Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors
Properties of Semiconductor Alloys: Group...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

Wiley Series in Materials for Electronic & Optoelectronic Applications Series Editors Peter Capper, SELEX Sensors and Airborne Systems Infrared Ltd, Southampton, UK Safa Kasap, University of Saskatchewan, Canada Arthur Willoughby, University of Southampton, Southampton, UK Published titles Bulk Crystal Growth of Electronic, Optical and Optoelectronic Materials, Edited by P. Capper Properties of Group-IV, III–V and II–VI Semiconductors, S. Adachi Charge Transport in Disordered Solids with Applications in Electronics, Edited by S. Baranovski Optical Properties of Condensed Matter and Applications, Edited by J. Singh Thin Film Solar Cells: Fabrication, Characterization and Applications, Edited by J. Poortmans and V. Arkhipov Dielectric Films for Advanced Microelectronics, Edited by M. R. Baklanov, M. Green and K. Maex Liquid Phase Epitaxy of Electronic, Optical and Optoelectronic Materials, Edited by P. Capper and M. Mauk Molecular Electronics: From Principles to Practice, M. Petty Luminescent Materials and Applications, Edited by A. Kitai CVD Diamond for Electronic Devices and Sensors, Edited by R. S. Sussman Forthcoming Titles Zinc Oxide Materials for Electronic and Optoelectronic Device Applications, Edited by C. Litton, D. C. Reynolds and T. C. Collins Mercury Cadmium Telluride: Growth, Properties and Applications, Edited by P. Capper and J. Garland Photovoltaic Materials: From Crystalline Silicon to Third-Generation Approaches, Edited by G. J. Conibeer Silicon Photonics: Fundamentals and Devices, J. Deen and P. K. Basu Inorganic Glasses for Photonics: Fundamentsls, Engineering and Applications, A. Jha, R. M. Almeida, M. Clara Goncalves and P. G. Kazansky

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors

SADAO ADACHI Gunma University, Gunma, Japan

This edition first published 2009 # 2009 John Wiley & Sons Ltd Registered office John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester, West Sussex, PO19 8SQ, United Kingdom For details of our global editorial offices, for customer services and for information about how to apply for permission to reuse the copyright material in this book please see our website at www.wiley.com. The right of the authors to be identified as the authors of this work has been asserted in accordance with the Copyright, Designs and Patents Act 1988. All rights reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted, in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, except as permitted by the UK Copyright, Designs and Patents Act 1988, without the prior permission of the publisher. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. Designations used by companies to distinguish their products are often claimed as trademarks. All brand names and product names used in this book are trade names, service marks, trademarks or registered trademarks of their respective owners. The publisher is not associated with any product or vendor mentioned in this book. This publication is designed to provide accurate and authoritative information in regard to the subject matter covered. It is sold on the understanding that the publisher is not engaged in rendering professional services. If professional advice or other expert assistance is required, the services of a competent professional should be sought. The publisher and the author make no representations or warranties with respect to the accuracy or completeness of the contents of this work and specifically disclaim all warranties, including without limitation any implied warranties of fitness for a particular purpose. This work is sold with the understanding that the publisher is not engaged in rendering professional services. The advice and strategies contained herein may not be suitable for every situation. In view of ongoing research, equipment modifications, changes in governmental regulations and the constant flow of information relating to the use of experimental reagents, equipment and devices, the reader is urged to review and evaluate the information provided in the package insert or instructions for each chemical, piece of equipment, reagent or device for, among other things, any changes in the instructions or indication of usage and for added warnings and precautions. The fact that an organization or Website is referred to in this work as a citation and/ or a potential source of further information does not mean that the author or the publisher endorses the information the organization or Website may provide or recommendations it may make. Further, readers should be aware that Internet Websites listed in this work may have changed or disappeared between when this work was written and when it is read. No warranty may be created or extended by any promotional statements for this work. Neither the publisher nor the author shall be liable for any damages arising herefrom. Library of Congress Cataloging-in-Publication Data Adachi, Sadao, 1950– Properties of semiconductor alloys : group-IV, III–V and II–VI semiconductors / Sadao Adachi. p. cm. Includes bibliographical references and index. ISBN 978-0-470-74369-0 1. Semiconductors–Materials. 2. Semiconductors–Analysis. 3. Silicon alloys. I. Title. TK7871.85.A32 2009 2008046980 621.38150 2–dc22 A catalogue record for this book is available from the British Library. ISBN 978-0-470-74369-0 (HB) Typeset in 10/12pt Times by Thomson Digital, Noida, India. Printed and bound in Great Britain by CPI Antony Rowe, Ltd, Chippenham, Wiltshire Front cover image of a photodiode array reproduced by kind permission of Dr. Jian-young Wu. Courtesy of Wutech Instruments and RedShirtImaging.

Contents Series Preface

xvii

Preface

xix

Abbreviations and Acronyms

xxi

Introductory Remarks A.1 An Alloy and a Compound A.2 Grimm–Sommerfeld Rule A.3 An Interpolation Scheme References 1 Structural Properties 1.1 Ionicity 1.2 Elemental Isotopic Abundance and Molecular Weight 1.3 Crystal Structure 1.3.1 Random Alloy 1.3.2 Spontaneous Ordering (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 1.4 Lattice Constant and Related Parameters 1.4.1 CuAu Alloy: Ordered and Disordered States 1.4.2 Non-alloyed Semiconductor 1.4.3 Semiconductor Alloy (a) Group-IV Semiconductor (b) III–V Semiconductor (c) II–VI Semiconductor 1.5 Coherent Epitaxy and Strain Problem 1.5.1 Bilayer Model 1.5.2 Elastic Strain and Lattice Deformation 1.5.3 Critical Thickness 1.6 Structural Phase Transition 1.7 Cleavage Plane 1.7.1 Cleavage 1.7.2 Surface Energy References

1 1 2 4 7 9 9 9 11 11 11 11 14 15 15 15 16 19 19 22 29 32 32 33 37 39 41 41 41 42

vi

CONTENTS

2 Thermal Properties 2.1 Melting Point and Related Parameters 2.1.1 Phase Diagram (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 2.1.2 Melting Point 2.2 Specific Heat 2.2.1 Group-IV Semiconductor Alloy 2.2.2 III–V Semiconductor Alloy 2.2.3 II–VI Semiconductor Alloy 2.3 Debye Temperature 2.3.1 General Considerations 2.3.2 Group-IV Semiconductor Alloy 2.3.3 III–V Semiconductor Alloy 2.3.4 II–VI Semiconductor Alloy 2.4 Thermal Expansion Coefficient 2.4.1 Group-IV Semiconductor Alloy 2.4.2 III–V Semiconductor Alloy 2.4.3 II–VI Semiconductor Alloy 2.5 Thermal Conductivity and Diffusivity 2.5.1 Thermal Conductivity (a) General Considerations (b) Group-IV Semiconductor Alloy (c) III–V Semiconductor Alloy (d) II–VI Semiconductor Alloy 2.5.2 Thermal Diffusivity (a) General Considerations (b) Alloy Value References

45 45 45 45 45 48 51 51 51 54 56 56 56 57 58 58 59 59 61 63 63 63 63 66 68 74 75 75 75 76

3 Elastic Properties 3.1 Elastic Constant 3.1.1 General Considerations 3.1.2 Room-temperature Value (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 3.1.3 External Perturbation Effect (a) Temperature Effect (b) Pressure Effect 3.2 Third-order Elastic Constant 3.3 Young’s Modulus, Poisson’s Ratio and Similar Properties 3.3.1 Group-IV Semiconductor Alloy 3.3.2 III–V Semiconductor Alloy 3.3.3 II–VI Semiconductor Alloy

81 81 81 81 81 81 84 86 86 88 89 89 89 89 90

CONTENTS

3.4

Microhardness 3.4.1 Group-IV Semiconductor Alloy 3.4.2 III–V Semiconductor Alloy 3.4.3 II–VI Semiconductor Alloy 3.5 Sound Velocity References

vii

92 92 92 93 96 97

4 Lattice Dynamic Properties 4.1 Phonon Dispersion Relationships 4.2 Phonon Frequency 4.2.1 General Considerations 4.2.2 Room-temperature Value (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 4.2.3 External Perturbation Effect (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 4.3 Mode Gr€ uneisen Parameter 4.3.1 Phonon Deformation Potential References

99 99 99 99 100 100 104 109 112 112 113 115 119 121 123

5 Collective Effects and Some Response Characteristics 5.1 Piezoelectric Constant 5.1.1 General Considerations 5.1.2 Alloy Value 5.2 Fr€ ohlich Coupling Constant 5.2.1 General Considerations 5.2.2 Alloy Value References

125 125 125 125 129 129 129 131

6 Energy-band Structure: Energy-band Gaps 6.1 Introductory Remarks 6.1.1 Quasi-cubic Band Model 6.1.2 Bowing Parameter 6.1.3 Ordered Alloy 6.2 Group-IV Semiconductor Alloy 6.2.1 Binary Alloy (a) CSi (b) CGe (c) SiGe (d) GeSn 6.2.2 Ternary Alloy (a) CSiGe (b) SiGeSn 6.2.3 Summary

133 133 133 136 136 139 139 139 140 141 144 145 145 147 147

viii

6.3

6.4

CONTENTS

III–V Semiconductor Ternary Alloy 6.3.1 (III, III)–N Alloy (a) c-AlGaN (b) w-AlGaN (c) c-AlInN (d) w-AlInN (e) c-GaInN (f) w-GaInN 6.3.2 (III, III)–P Alloy (a) AlGaP (b) AlInP (c) GaInP 6.3.3 (III, III)–As Alloy (a) AlGaAs (b) AlInAs (c) GaInAs 6.3.4 (III, III)–Sb Alloy (a) AlGaSb (b) AlInSb (c) GaInSb 6.3.5 Dilute-nitride III–(V, V) Alloy (a) General Considerations (b) GaNP (c) GaNAs (d) GaNSb (e) InNP (f) InNAs (g) InNSb 6.3.6 Al–(V, V) Alloy 6.3.7 Ga–(V, V) Alloy (a) GaPAs (b) GaPSb (c) GaAsSb 6.3.8 In–(V, V) Alloy (a) InPAs (b) InPSb (c) InAsSb 6.3.9 Summary III–V Semiconductor Quaternary Alloy 6.4.1 Dilute-nitride Quaternary Alloy (a) AlGaNAs (b) GaInNP (c) GaInNAs (d) GaNPAs 6.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs (b) AlGaAsSb

149 149 149 150 152 152 152 152 153 153 153 155 157 157 160 161 163 163 165 166 166 166 170 171 172 173 173 174 174 175 175 176 178 179 179 179 181 183 184 184 184 185 185 185 186 186 187

CONTENTS

6.4.3

6.5

6.4.4 6.4.5 II–VI 6.5.1

6.5.2

6.5.3

6.5.4

6.5.5

6.5.6

6.5.7

6.5.8

(c) AlInAsSb (d) GaInPAs (e) GaInAsSb (III, III, III)–V Alloy (a) AlGaInP (b) AlGaInAs III–(V, V, V) Alloy Summary Semiconductor Alloy (II, II)–O Ternary Alloy (a) BeZnO (b) MgZnO (c) ZnCdO (II, II)–S Ternary Alloy (a) MgZnS (b) ZnCdS (c) ZnHgS (d) CdHgS (II, II)–Se Ternary Alloy (a) BeZnSe (b) BeCdSe (c) MgZnSe (d) MgCdSe (e) ZnCdSe (f) CdHgSe (II, II)–Te Ternary Alloy (a) BeZnTe (b) MgZnTe (c) MgCdTe (d) ZnCdTe (e) ZnHgTe (f) CdHgTe Zn–(VI, VI) Ternary Alloy (a) ZnOS (b) ZnOSe (c) ZnSSe (d) ZnSTe (e) ZnSeTe Cd–(VI, VI) Ternary Alloy (a) CdSSe (b) CdSTe (c) CdSeTe (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe (b) MgZnSeTe (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe

ix

188 189 191 193 193 194 195 196 197 197 197 197 198 198 198 200 200 200 201 201 202 202 202 203 203 204 204 205 206 206 207 208 208 208 209 209 210 210 210 210 211 211 212 212 213 213 213

x

CONTENTS

(b) BeZnCdSe (c) MgZnCdSe Summary

213 214 214 216

7 Energy-band Structure: Effective Masses 7.1 Introductory Remarks 7.1.1 Electron Effective Mass 7.1.2 Hole Effective Mass 7.1.3 Interpolation Scheme 7.2 Group-IV Semiconductor Alloy 7.2.1 CSi Binary Alloy 7.2.2 SiGe Binary Alloy 7.3 III–V Semiconductor Ternary Alloy 7.3.1 (III, III)–N Alloy 7.3.2 (III, III)–P Alloy 7.3.3 (III, III)–As Alloy (a) AlGaAs (b) AlInAs (c) GaInAs 7.3.4 (III, III)–Sb Alloy 7.3.5 Dilute-nitride III–(V, V) Alloy (a) Ga–(N, V) Alloy (b) In–(N, V) Alloy 7.3.6 Al–(V, V) Alloy 7.3.7 Ga–(V, V) Alloy (a) GaPAs (b) GaAsSb 7.3.8 In–(V, V) Alloy (a) InPAs (b) InAsSb 7.4 III–V Semiconductor Quaternary Alloy 7.4.1 Dilute-nitride Quaternary Alloy 7.4.2 (III, III)–(V, V) Alloy (a) GaInPAs (b) GaInAsSb 7.4.3 (III, III, III)–V Alloy (a) AlGaInP (b) AlGaInAs 7.4.4 III–(V, V, V) Alloy 7.5 II–VI Semiconductor Alloy 7.5.1 (II, II)–VI Ternary Alloy 7.5.2 II–(VI, VI) Ternary Alloy 7.5.3 (II, II)–(VI, VI) Quaternary Alloy 7.6 Concluding Remarks 7.6.1 Composition Dependence 7.6.2 External Perturbation Effect References

229 229 229 230 232 234 234 237 238 238 238 239 239 241 241 242 243 243 244 245 245 245 246 246 246 247 248 248 248 248 249 250 250 250 250 251 251 253 253 254 254 254 256

6.5.9 References

CONTENTS

8 Deformation Potentials 8.1 Intravalley Deformation Potential: Point 8.1.1 Group-IV Semiconductor Alloy 8.1.2 III–V Semiconductor Ternary Alloy (a) AlGaN (b) GaInN (c) AlInP (d) GaInP (e) AlGaAs (f) AlInAs (g) GaInAs (h) GaNAs (i) GaPAs 8.1.3 III–V Semiconductor Quaternary Alloy 8.1.4 II–VI Semiconductor Alloy 8.2 Intravalley Deformation Potential: High-symmetry Points 8.2.1 Group-IV Semiconductor Alloy 8.2.2 III–V Semiconductor Alloy 8.2.3 II–VI Semiconductor Alloy 8.3 Intervalley Deformation Potential 8.3.1 Group-IV Semiconductor Alloy 8.3.2 III–V Semiconductor Alloy 8.3.3 II–VI Semiconductor Alloy References 9 Heterojunction Band Offsets and Schottky Barrier Height 9.1 Heterojunction Band Offsets 9.1.1 General Considerations 9.1.2 Group-IV Semiconductor Heterostructure System (a) CSi/Si (b) SiGe/Si (c) CSiGe/Si (d) CSi/SiGe 9.1.3 III–V Semiconductor Heterostructure System: Lattice-matched Ternary-alloy System (a) GaInP/GaAs (b) GaInP/AlInP (c) GaInP/AlGaAs (d) AlGaAs/GaAs (e) AlInAs/InP (f) GaInAs/InP (g) GaInAs/AlInAs (h) InAsSb/GaSb 9.1.4 III–V Semiconductor Heterostructure System: Lattice-matched Quaternary Alloy (a) GaInPAs/InP

xi

259 259 259 261 261 262 262 263 263 264 265 265 266 266 266 267 267 269 270 270 270 271 272 272

275 275 275 275 275 276 276 277 277 277 277 278 278 279 279 280 280 280 280

xii

CONTENTS

(b) AlGaAsSb/GaSb (c) AlGaAsSb/InP (d) AlGaAsSb/InAs (e) GaInAsSb/GaSb (f) GaInAsSb/InP (g) GaInAsSb/InAs (h) AlGaAsSb/GaInAsSb (i) AlInAsSb/GaInAsSb (j) AlGaInP/AlInP (k) AlGaInP/GaInP (l) AlGaInAs/GaInAs 9.1.5 III–V Semiconductor Heterostructure System: Lattice-mismatched Alloy System (a) w-AlGaN/w-GaN (b) w-AlInN/w-InN (c) w-GaInN/w-GaN (d) GaInAs/GaAs (e) Dilute-nitride-based Heterostructure System 9.1.6 II–VI Semiconductor Heterostructure System (a) (II, II)–O-based Heterostructure System (b) (II, II)–S-based Heterostructure System (c) (II, II)–Se-based Heterostructure System (d) (II, II)–Te-based Heterostructure System (e) Zn–(VI, VI)-based Heterostructure System (f) (II, II)–VI-based and II–(VI, VI)-based Heterostructure Systems (g) (II, II)–(VI, VI)-based Heterostructure System (h) (II, II, II)–VI-based Heterostructure System 9.2 Schottky Barrier Height 9.2.1 General Considerations 9.2.2 Group-IV Semiconductor Alloy (a) SiGe Binary Alloy (b) CSiGe Ternary Alloy 9.2.3 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) (III, III)–Sb Alloy (e) Ga–(V, V) Alloy 9.2.4 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) Alloy (b) (III, III, III)–V Alloy 9.2.5 II–VI Semiconductor Alloy (a) (II, II)–Te Ternary Alloy (b) Zn–(VI, VI) Ternary Alloy References

281 281 281 281 281 281 282 282 282 282 283 283 283 284 284 284 286 287 287 287 287 288 289 289 289 289 289 289 290 290 291 291 291 292 292 294 295 296 296 297 299 299 300 300

CONTENTS

10 Optical Properties 10.1 Introductory Remarks 10.1.1 Optical Dispersion Relations 10.1.2 Static and High-frequency Dielectric Constants 10.2 Group-IV Semiconductor Alloy 10.2.1 Binary Alloy (a) CSi (b) CGe (c) SiGe (d) GeSn 10.2.2 Ternary Alloy 10.3 III–V Semiconductor Ternary Alloy 10.3.1 (III, III)–N Alloy (a) c-(III, III)–N Alloy (b) w-AlGaN (c) w-AlInN (d) w-GaInN 10.3.2 (III, III)–P Alloy (a) AlGaP (b) AlInP (c) GaInP 10.3.3 (III, III)–As Alloy (a) AlGaAs (b) AlInAs (c) GaInAs 10.3.4 (III, III)–Sb Alloy (a) AlGaSb (b) GaInSb 10.3.5 Dilute-nitride III–(V, V) Alloy (a) GaNP (b) GaNAs (c) GaNSb (d) InNP (e) InNAs 10.3.6 Al–(V, V) Alloy 10.3.7 Ga–(V, V) Alloy (a) GaPAs (b) GaPSb (c) GaAsSb 10.3.8 In–(V, V) Alloy (a) InPAs (b) InPSb (c) InAsSb 10.4 III–V Semiconductor Quaternary Alloy 10.4.1 Dilute-nitride Quaternary Alloy (a) GaInNP (b) GaInNAs

xiii

307 307 307 308 308 308 308 309 309 310 311 311 311 311 312 313 313 314 314 314 315 316 316 316 318 319 319 319 320 320 321 321 322 322 322 323 323 324 324 324 324 325 325 326 326 326 326

xiv

CONTENTS

10.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs (b) AlGaAsSb (c) GaInPAs (d) GaInAsSb 10.4.3 (III, III, III)–V Alloy (a) AlGaInP (b) AlGaInAs 10.4.4 III–(V, V, V) Alloy 10.5 II–VI Semiconductor Alloy 10.5.1 (II, II)–O Ternary Alloy (a) BeZnO (b) MgZnO (c) ZnCdO 10.5.2 (II, II)–S Ternary Alloy (a) MgZnS (b) ZnCdS 10.5.3 (II, II)–Se Ternary Alloy (a) BeZnSe (b) BeCdSe (c) MgZnSe (d) MgCdSe (e) ZnCdSe (f) CdHgSe 10.5.4 (II, II)–Te Ternary Alloy (a) BeZnTe (b) MgZnTe (c) MgCdTe (d) ZnCdTe (e) ZnHgTe (f) CdHgTe 10.5.5 Zn–(VI, VI) Ternary Alloy (a) ZnOS (b) ZnSSe (c) ZnSTe (d) ZnSeTe 10.5.6 Cd–(VI, VI) Ternary Alloy (a) CdSSe (b) CdSTe (c) CdSeTe 10.5.7 (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe (b) MgZnSeTe 10.5.8 (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe (b) BeZnCdSe (c) MgZnCdSe References

326 326 327 327 328 330 330 331 332 332 332 332 332 333 333 333 334 335 335 335 335 337 337 338 339 339 339 340 340 342 342 343 343 343 343 344 344 344 345 346 346 346 346 346 346 346 346 347

CONTENTS

xv

11 Elasto-optic, Electro-optic and Nonlinear Optical Properties 11.1 Elasto-optic Effect 11.1.1 Group-IV Semiconductor Alloy 11.1.2 III–V Semiconductor Alloy 11.1.3 II–VI Semiconductor Alloy 11.2 Linear Electro-optic Constant 11.2.1 Group-IV Semiconductor Alloy 11.2.2 III–V Semiconductor Alloy 11.2.3 II–VI Semiconductor Alloy 11.3 Quadratic Electro-optic Constant 11.3.1 Group-IV Semiconductor Alloy 11.3.2 III–V Semiconductor Alloy 11.3.3 II–VI Semiconductor Alloy 11.4 Franz–Keldysh Effect 11.4.1 Group-IV Semiconductor Alloy 11.4.2 III–V Semiconductor Alloy 11.4.3 II–VI Semiconductor Alloy 11.5 Nonlinear Optical Constant 11.5.1 Group-IV Semiconductor Alloy 11.5.2 III–V Semiconductor Alloy 11.5.3 II–VI Semiconductor Alloy References

357 357 357 357 357 358 358 358 358 360 360 360 360 360 360 360 360 361 361 361 362 362

12 Carrier Transport Properties 12.1 Introductory Remarks 12.2 Low-field Mobility 12.2.1 Group-IV Semiconductor Alloy (a) CSi Binary Alloy (b) SiGe Binary Alloy 12.2.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) (III, III)–Sb Alloy (e) Dilute-nitride III–(V, V) Alloy (f) Ga–(V, V) Alloy (g) In–(V, V) Alloy 12.2.3 III–V Semiconductor Quaternary Alloy (a) Dilute-nitride Alloy (b) (III, III)–(V, V) Alloy (c) (III, III, III)–V Alloy 12.2.4 II–VI Semiconductor Alloy (a) (II, II)–O Ternary Alloy (b) (II, II)–Se Ternary Alloy (c) (II, II)–Te Ternary Alloy (d) Zn–(V, V) Ternary Alloy

365 365 367 367 367 367 368 368 369 369 369 371 371 371 371 371 372 373 374 374 374 375 376

xvi

CONTENTS

12.3 High-field Transport 12.3.1 Group-IV Semiconductor Alloy 12.3.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) Dilute-nitride III–(V, V) Alloy 12.3.3 III–V Semiconductor Quaternary Alloy 12.3.4 II–VI Semiconductor Alloy 12.4 Minority-carrier Transport 12.4.1 Group-IV Semiconductor Alloy (a) SiGe Binary Alloy (b) CSiGe Ternary Alloy 12.4.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–As Alloy (c) Ga–(V, V) Alloy 12.4.3 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) Alloy (b) (III, III, III)–V Alloy 12.4.4 II–VI Semiconductor Alloy 12.5 Impact Ionization Coefficient 12.5.1 Group-IV Semiconductor Alloy 12.5.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) (III, III)–Sb Alloy (e) Dilute-nitride III–(V, V) Alloy (f) Ga–(V, V) Alloy (g) In–(V, V) Alloy 12.5.3 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) Alloy (b) (III, III, III)–V Alloy 12.5.4 II–VI Semiconductor Alloy References Index

376 376 376 376 376 377 378 378 379 379 379 379 380 380 380 380 381 381 381 382 382 382 382 382 382 383 383 384 384 385 385 385 385 385 386 386 391

Preface Semiconductor alloys provide a natural means of tuning the magnitude of the band-gap energy and other material properties so as to optimize and widen the application of semiconductor devices. Current research and development in semiconductor alloys is focused on areas of improved materials growth, development of unique materials characterization and suitable process technologies, fabrication of novel devices using artificially controlled materials structures and better understanding of degradation mechanisms in electronic and optoelectronic devices for improved device reliability. Even though the basic semiconductor alloy concepts are understood at this time, the determination of some device parameters has been hampered by a lack of definite knowledge of many material parameters. The main purpose of this book is to provide a comprehensive treatment of the materials aspects of group-IV, III V and II VI semiconductor alloys used in various electronic and optoelectronic devices. The topics treated in this book include the structural, thermal, mechanical, lattice vibronic, electronic, optical and carrier transport properties of such semiconductor alloys. The book covers not only commonly known alloys (SiGe, AlGaAs, GaInPAs, ZnCdTe, etc.) but also new alloys, such as dilute-carbon alloys (CSiGe, CSiSn, etc.), III N alloys, dilute-nitride alloys (GaNAs, GaInNAs, etc.) and Mg- or Be-based II VI semiconductor alloys. The reader may also find the companion book Properties of Group-IV, III V and II VI Semiconductors published in this series useful since it emphasizes the endpoint semiconductor principles and properties. The extensive bibliography is included for those who wish to find additional information if required. It is hoped that the book will attract the attention of not only semiconductor device engineers, but also solid-state physicists and materials scientists, and particularly postgraduate students, R&D staff and teaching and research professionals. Sadao Adachi, Gunma University, Japan

Series Preface WILEY SERIES IN MATERIALS FOR ELECTRONIC AND OPTOELECTRONIC APPLICATIONS This book series is devoted to the rapidly developing class of materials used for electronic and optoelectronic applications. It is designed to provide much-needed information on the fundamental scientific principles of these materials, together with how these are employed in technological applications. The books are aimed at (postgraduate) students, researchers and technologists, engaged in research, development and the study of materials in electronics and photonics, and industrial scientists developing new materials, devices and circuits for the electronic, optoelectronic and communications industries. The development of new electronic and optoelectronic materials depends not only on materials engineering at a practical level, but also on a clear understanding of the properties of materials, and the fundamental science behind these properties. It is the properties of a material that eventually determine its usefulness in an application. The series therefore also includes such titles as electrical conduction in solids, optical properties, thermal properties, and so on, all with applications and examples of materials in electronics and optoelectronics. The characterization of materials is also covered within the series in as much as it is impossible to develop new materials without the proper characterization of their structure and properties. Structure-property relationships have always been fundamentally and intrinsically important to materials science and engineering. Materials science is well known for being one of the most interdisciplinary sciences. It is the interdisciplinary aspect of materials science that has led to many exciting discoveries, new materials and new applications. It is not unusual to find scientists with a chemical engineering background working on materials projects with applications in electronics. In selecting titles for the series, we have tried to maintain the interdisciplinary aspect of the field, and hence its excitement to researchers in this field. Peter Capper Safa Kasap Arthur Willoughby

Abbreviations and Acronyms BAC bct BZ

band anticrossing body-centered tetragonal Brillouin zone

cCB CL Cl-VPE CP CR C–V CVD

cubicconduction band cathodoluminescence chloride-transport vapor-phase epitaxy critical point cyclotron resonance capacitance–voltage chemical vapor deposition

DLTS DOS DP

deep-level transient spectroscopy density of states deformation potential

ER EXAFS

electroreflectance extended X-ray absorption fine-structure spectroscopy

fcc FET FTIR

face-centered cubic field effect transistor Fourier transform infrared

HBT HH HREELS HRXRD HT-VPE

heterojunction bipolar transistor heavy-hole high-resolution electron-energy-loss spectroscopy high-resolution X-ray diffraction hydride-transport vapor-phase epitaxy

IR I–V

infrared current–voltage

LA LH LO LPE

longitudinal acoustic light-hole longitudinal optical liquid-phase epitaxy

MBE MDF MOCVD

molecular beam epitaxy model dielectric function metalorganic chemical vapor deposition

xxii

ABBREVIATIONS AND ACRONYMS

MOMBE MQW MREI

metalorganic molecular beam epitaxy multiple quantum well modified random-element-isodisplacement

PDP PIXE PL PLD PLE PR PzR

phonon deformation potential particle-induced X-ray emission photoluminescence pulsed-laser deposition photoluminescence excitation photoreflectance piezoreflectance

QW

quantum well

RBS rf RHEED

Rutherford backscattering spectrometry radio-frequency reflection high-energy electron diffraction

SE SL SO

spectroscopic ellipsometry superlattice spin–orbit

TA TEM THM TO TP TR

transverse acoustic transmission electron microscopy traveling heater method transverse optical triple-period thermoreflectance

UHV UV

ultrahigh vacuum ultraviolet

VB VCA VPE

valence band virtual crystal approximation vapor-phase epitaxy

wWDXS

wurtzite wavelength-dispersive X-ray spectroscopy

XPS XRD

X-ray photoelectron spectroscopy X-ray diffraction

1D 2D 3D

one-dimensional two-dimensional three-dimensional

Introductory Remarks A.1 AN ALLOY AND A COMPOUND An alloy is a combination, either in solution or compound, of two or more elements. An alloy with two components is called a binary alloy; one with three is a ternary alloy; one with four is a quaternary alloy; one with five is a pentanary alloy. The resulting alloy substance generally has properties significantly different from those of its components. The proportions of the ingredients are available. A chemical compound is a substance consisting of two or more chemical elements that are chemically combined in fixed proportions. The ratio of each element is usually expressed by chemical formula. For example, water is a compound consisting of two hydrogen atoms bonded to an oxygen atom (H2O). The atoms within a compound can be held together by a variety of interactions, ranging from covalent bonds to electrostatic forces in ionic bonds. A continuum of bond polarities exists between the purely covalent and ionic bonds. For example, H2O is held together by polar covalent bonds. NaCl is an example of an ionic compound. Simply, an alloy is formed from a physical mixture of two or more substances, while a compound is formed from a chemical reaction. An alloy crystal is sometimes called a mixed crystal or a solid solution. For example, GaAs is a compound consisting of Ga atoms bonded to As atoms. It is not an alloy. AlxGa1xAs is an alloy compound consisting of AlAs and GaAs with a mole ratio of x:(1 x). The bonds in GaAs and AlAs are not adequately described by any of these extreme types, but have characteristics intermediate to those usually associated with the covalent and ionic terms. The bonds in diamond, CC, can be described by the covalent bond term only. It is an elemental semiconductor, not a compound semiconductor. Similarly, Si and Ge are elemental semiconductors. Like AlxGa1xAs, SixGe1x (0 x 1.0) is an alloy semiconductor. The bonds SiGe, SiSi and GeGe in SixGe1x are, therefore, described by the covalent term only. It should be noted, however, that silicon carbide (SiC) is a compound, not an alloy. This is because that the chemical bonds in SiC cannot be described only by the covalent term, but have characteristics intermediate to those associated with the covalent and ionic terms, like GaAs and AlAs. There is an ordered alloy phase in SixGe1x binary alloy [1]. This phase exhibits long-range order rather than random arrangement of atoms as expected previously. The ordered phase, as expected, occurs mostly in bulk SixGe1x layers at x 0.5 and can be explained by the rhombohedral structure. Note that SiC is thought to be an ordered alloy. It crystallizes in a large number of polytypes. The various types of SiC differ one from another only by the order in which successive planes of Si (or C) atoms are stacked along the c axis; one polytype is the cubic, zinc-blende structure (3C) while the reminder, including two of the more frequently occurring forms, 6H (hexagonal) and 15R (rhombohedral), possess uniaxial symmetry [2]. There is no diamond structure in the SiC polytypes. An ordered alloy phase has been found not only in SixGe1x, but also in many III–V and II–VI semiconductor alloys [3]. Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

2

PROPERTIES OF SEMICONDUCTOR ALLOYS

A.2 GRIMM–SOMMERFELD RULE The periodic law is most commonly expressed in chemistry in the form of a periodic table or chart. An important part of this table is shown in Table A.1. The so-called short-form periodic table, based on the Mendeleyev table, with subsequent emendations and additions, is still in widespread use. The elements in this table are arranged in seven horizontal rows, called the periods, in order of increasing atomic weights, and in 18 vertical columns, called the groups. The first period, containing two elements, H and He, and the next two periods, each containing eight elements, are called the short periods. The remaining periods, called the long periods, contain 18 elements, as in periods 4 and 5, or 32 elements, as in period 6. The long period 7 includes the actinide series, which has been filled in by the synthesis of radioactive nuclei through element 103, lawrencium (Lr). Heavier transuranium elements, atomic numbers 104 to 112, have also been synthesized. Table A.1 Periodic table

The elemental semiconductors in column IVa of the periodic table are diamond, Si and Ge, and they are of some importance in various device applications. Note that gray tin (a-Sn) is a semiconductor (semimetal) and Pb is a metal. SiC is the only compound semiconductor formed by column IVa elements. The III–V and II–VI semiconductors possess a crystal structure similar to either one of the cubic mineral, sphalerite or to hexagonal wurtzite. There are 15 III–V, 18 II–VI and four I–VII compound semiconductors. The four I–VII compound semiconductors are: CuCl, CuBr, CuI and AgI. A substantial development in the search for semiconducting materials with new combinations of physical and chemical properties was reached when Goryunova using the ideas of Huggins [4] and Grimm and Sommerfeld [5], developed a method of prediction of the composition of chemical compounds with the tetrahedral and octahedral (NaCl-type) coordination of atoms in their crystal lattice [6]. His method is based on consideration of the number of valence electrons in the elements, which is assumed to be equal to the number of the group in

INTRODUCTORY REMARKS

3

the periodic table to which they belong (so-called full or normal valency) and can be expressed in the form of the equation system [7] A X i¼1 n X i¼1 A X

Bi x i ¼ 4 Bi x i ¼

A X

ð8Bi Þxi

ðA:1Þ

i¼nþ1

xi ¼ 1

i¼1

for calculating the content of the representatives of different groups of the periodic table in a compound containing A components, n of which are considered as cations, where Bi is the number of the group in the periodic table to which the ith component of the compounds belongs, and xi is its concentration in the compound. The first expression in Equation (A.1) represents the condition that the average number of valence electrons per atom is equal to four (tetrahedral rule). The second equation states that in the compound, the number of valence electrons, which cations give to anions is equal to the number of electrons the anion needs to form the octet (i.e. the normal valency condition). The quotation marks here are used to remind us that in the solids with dominating covalent bonds, which factually form the class of semiconductor, the ion concept is quite conditional. Based on these criteria, it is possible to obtain all probable types of tetrahedral substances, taking into consideration only the location of their components in one or another group of the periodic table. Table A.2 briefly summarizes these results. Table A.2 Summary of valence binary compounds and ternary analogs of binary valence compounds which satisfy tetrarahedral rule (Z¼4). ch¼chalcopyrite; zb¼zinc-blende; t¼tetragonal; or¼orthorhombic; w¼wurtzite; h¼hexagonal (P63mc (C6v)); rh¼rhombohedral Cation

Compound

Typical compound (Crystal structure)

I

I–III–VI2 I–IV2–V3 I2–IV–VI3 I3–V–VI4 I–VII

CuGaSe2 (ch) CuGe2P3 (zb) Cu2GeSe3 (t) Cu3PS4 (or) g-CuCl (w)

II

II4–III–VII3 II–IV–V2 II3–IV–VII2 II2–V–VII II–VI

III

IV

ZnSiP2 (ch) CdTe (zb)

III2–IV–VI III3–IV2–VII III–V

GaAs (zb)

IV–IV

SiC (zb, w, h, rh)

Al2CO (w)

4

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table A.3 All the possible types of valence binary compound Cation

Cation to anion content ratio x/y, (Z), Typical compound II

I

6:1 (1.14)

III

IV

V

5:1 (1.33)

4:1 (1.60)

5:2 (2.29)

2:1 (2.67) Mg2Si 4:3 (3.43)

II

—

III

—

—

IV

—

—

V

—

—

VI

—

—

1:1 (4.00) SiC — —

3:1 (2.00) K3Sb 3:2 (3.20) Cd3As2 1:1 (4.00) GaAs 3:4 (4.57) — —

VI 2:1 (2.67) Ag2S 1:1 (4.00) CdTe 2:3 (4.80) Ga2Se3 1:2 (5.33) SnS2 2:5 (5.71) —

VII 1:1 (4.00) g-CuCl 1:2 (5.33) HgI2 1:3 (6.00) 1:4 (6.40) 1:5 (6.67) 1:6 (6.86)

In analyzing the normal valency compounds, not only tetrahedral phases but all compounds of this category can be grouped, first of all, in accordance with the average valence electron content per atom of a compound, Z. We list in Table A.3 all possible types of the binary valence compounds [7]. If A and B are the cation valencies in a binary compound, the atomic ratio of components in a valence compound AxBy is given by x 8B ¼ y A

ðA:2Þ

and the valence electron concentration per atom in the corresponding binary compound is Z¼

8A 8A ¼ 8ðBAÞ 8þðABÞ

ðA:3Þ

as following from Equation (A.1). In Table A.3, there are 22 types of binary valence compounds. Goryunova [6] concluded from the available experimental data that the phases possessing semiconducting properties are those with Z between two and six; the phases smaller than two are either metal alloys or the compounds with typical metallic crystal structure and properties. Goryunova also showed that there are 148 types of ternary compounds which are the electron analogs of the binary valence compounds [7]. Among them, there are 10 types of ternary compounds which satisfy the tetrarahedral rule Z ¼ 4, as listed in Table A.2.

A.3 AN INTERPOLATION SCHEME The electronic energy-band parameters of semiconductor alloys and their dependence on alloy compositionareveryimportant,andsotheyhavereceivedmuchattentioninthepast.Investigation

INTRODUCTORY REMARKS

5

of many device parameters have, however, been hampered by a lack of definite knowledge of various material parameters. This necessitates the use of some sort of interpolation scheme. If the linear interpolation scheme is used, the ternary material parameter T for an alloy of the form AxB1xC can be derived from binary parameters (B) by TðxÞ ¼ xBAC þð1xÞBBC aþbx

ðA:4Þ

where a BBC and b BAC BBC. Some material parameters, however, deviate significantly from the linear relationship shown in Equation (A.4), and exhibit an approximately quadratic dependence on x. The ternary material parameter in such a case can be very efficiently approximated by the relationship TðxÞ ¼ xBAC þð1xÞBBC þxð1xÞCAB aþbxþcx2

ðA:5Þ

where a BBC, b BAC BBC þ CAB and c CAB. The parameter c is called a bowing parameter. The quaternary material AxB1xCyD1y is thought to be constructed from four binaries: AC, AD, BC and BD. If the linear interpolation scheme is used, the quaternary material parameter Q can be derived from the binary parameters by Qðx;yÞ ¼ xyBAC þxð1yÞBAD þð1xÞyBBC þð1xÞð1yÞBBD

ðA:6Þ

If one of the four binary parameters (e.g. BAD) is lacking, Q can be estimated from Qðx;yÞ ¼ xBAC þðyxÞBBC þð1yÞBBD

ðA:7Þ

The quaternary material AxByC1xyD is thought to be constructed from three binaries: AD, BD and CD. The corresponding linear interpolation is given by Qðx;yÞ ¼ xBAD þyBBD þð1xyÞBCD

ðA:8Þ

If relationships for the ternary parameters are available, the quaternary material parameter Q can be expressed either as (AxB1xCyD1y) Qðx;yÞ ¼

xð1xÞ½yTABC ðxÞþð1yÞTABD ðxÞþyð1yÞ½xTACD ðyÞþð1xÞTBCD ðyÞ xð1xÞþyð1yÞ

ðA:9Þ

or (AxByC1xyD) Qðx;yÞ ¼

xyTABD ðuÞþyð1xyÞTBCD ðvÞþxð1xyÞTACD ðwÞ xyþyð1xyÞþxð1xyÞ

ðA:10Þ

with u ¼ ð1xyÞ=2 v ¼ ð2x2yÞ=2 w ¼ ð22xyÞ=2

ðA:11Þ

6

PROPERTIES OF SEMICONDUCTOR ALLOYS

If a quaternary bowing term DABCD ¼ d is considered in Equation (A.9) or Equation (A.10), we can obtain Qðx;yÞ ¼ fxð1xÞ½yTABC ðxÞþð1yÞTABD ðxÞþyð1yÞDABCD þyð1yÞ ½xTACD ðyÞþð1xÞTBCD ðyÞþxð1xÞDABCD g½xð1xÞþyð1yÞ1

; ðA:12Þ

for the AxB1xCyD1y quaternary or Qðx;yÞ ¼

xyTABD ðuÞþyð1xyÞTBCD ðvÞþxð1xyÞTACD ðwÞþxyð1xyÞDABCD ðA:13Þ xyþyð1xyÞþxð1xyÞ

for the AxByC1xyD quaternary. The weighted form of Equation (A.12) can be written as Qðx;yÞ ¼ yð1xÞBBC þxyBAC þð1yÞxBAD þð1xÞð1yÞBCD þxð1xÞð1yÞCABðDÞ þxð1xÞyCABðCÞ þð1xÞyð1yÞCðBÞCD þxyð1yÞCðAÞCD þxð1xÞyð1yÞDABCD

ðA:14Þ

where CAB(D) is the ternary bowing parameter for an alloy AxB1xD and so on. Expression (A.14) can be conveniently compacted into an inner product whose 3 3 matrix includes only the alloy parameters and closely resembles the map of the quaternary alloy in its compositional space [8] 2 32 3 BBC CABðCÞ BAC 1x Qðx;yÞ ¼ ½ y yð1yÞ 1y 4 CðBÞCD DABCD CðAÞCD 54 xð1xÞ 5 ðA:15Þ BBD CABðDÞ BAD x If the bowing parameters C and D in Equation (A.15) are zero, Vegard law is recovered in its bilinear formulation. Equation (A.15) is valid for quaternaries of types AxB1xCyD1y and AxByC1xyD (ABxCyD1xy). For the latter, one binary can be assigned twice in the same raw or column of the alloy matrix with a zero bowing factor (i.e. BAC ¼ BAD and C(A)CD ¼ 0). The composition for such an alloy is given by (BAD)x[(BBD)y(BCD)1y]1x (e.g., Alx(GayIn1y)1xP). The essentially same expressions can be obtained for group-IV semiconductor alloys. The binary material parameter B in the form of AxB1x can be written using the elemental material parameters (A) as BðxÞ ¼ xAA þð1xÞAB aþbx

ðA:16Þ

The bowing effect modifies Equation (A.16) in the form BðxÞ ¼ xAA þð1xÞAB þxð1xÞCAB aþbxþcx2

ðA:17Þ

Similarly, the ternary material parameter T in AxByC1xy can be expressed as Tðx;yÞ ¼ xAA þyAB þð1xyÞAC

ðA:18Þ

INTRODUCTORY REMARKS

7

and Tðx;yÞ ¼

xyBAB ðuÞþyð1xyÞBBC ðvÞþxð1xyÞBAC ðwÞ xyþyð1xyÞþxð1xyÞ

ðA:19Þ

or Tðx;yÞ ¼

xyBAB ðuÞþyð1xyÞBBC ðvÞþxð1xyÞBAC ðwÞþxyð1xyÞCABC xyþyð1xyÞþxð1xyÞ

ðA:20Þ

with u, v and w given in Equation (A.11). In Equation (A.20), CABC is a ternary bowing parameter.

REFERENCES [1] W. J€ager, in Properties of Strained and Relaxed Silicon Germanium, EMIS Datareviews Series No. 12 (edited by E. Kasper), INSPEC, London, 1995, p. 53. [2] S. Adachi, Properties of Group-IV, III-V and II-VI Semiconductors. John Wiley & Sons, Ltd, Chichester, 2005. [3] A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys. Kluwer Academic, New York, 2002. [4] M. L. Huggins, Phys. Rev. 27, 286 (1926). [5] H. Grimm and A. Sommerfeld, Z. Phys. 36, 36 (1926). [6] N. A. Goryunova, The Chemistry of Diamond-Like Semiconductors. MIT Press, Cambridge, 1965. [7] L. I. Berger, Semiconductor Materials. CRC, Boca Raton, 1997. [8] G. P. Donati, R. Kaspi, and K. J. Malloy, J. Appl. Phys. 94, 5814 (2003).

1 Structural Properties 1.1 IONICITY Details of ionicity fi are given in Adachi [1]. Any given definition of ionicity is likely to be imperfect. We present in Table 1.1 fi values for a number of group-IV, III–V and II–VI semiconductors, including Be-based semiconductors and CdO. We have Phillips ionicity of fi ¼ 0 for all group-IV elemental semiconductors (diamond, Si, Ge and a-Sn) and fi > 0.9 for some alkali halides (NaCl, KCl, etc.). Figure 1.1(a) plots fi versus x for CxSi1x. Note that fi ¼ 0.177 for silicon carbide (SiC). This means that the bond character of SiC resembles that of III–V or II–VI semiconductors rather than of Si or diamond, so that its crystal structure must be zinc-blende, hexagonal or rhombohedral. Similarly, an ordered alloy of SixGe1x may have a nonzero fi value near the ordered-phase composition x 0.5. In fully disordered alloys (CxSi1x, SixGe1x, etc.), we should have fi ¼ 0 over the whole alloy range 0 x 1.0. The plots of fi versus x or y for AlxGa1xAs, GaxIn1xPyAs1y/InP and MgxZn1xSySe1y/GaAs are shown in Figure 1.1(b). These values are obtained from the linear interpolation of Equations (A.4) and (A.6) between the endpoint data in Table 1.1. The resulting fi versus x (y) plots can be expressed in the usual power form as fi ðxÞ ¼ 0:310 0:036x

ð1:1aÞ

fi ðyÞ ¼ 0:335 þ 0:065y þ 0:021y2

ð1:1bÞ

fi ðxÞ ¼ 0:630 þ 0:154x þ 0:003x2

ð1:1cÞ

for AlxGa1xAs, for GaxIn1xPyAs1y/InP and for MgxZn1xSySe1y/GaAs. The values of fi for fully disordered alloys should be safely estimated from the linear interpolation scheme.

1.2 ELEMENTAL ISOTOPIC ABUNDANCE AND MOLECULAR WEIGHT In Tables 1.2 and 1.3 of Adachi [1], the elements which form at least one tetrahedrally coordinated ANB8N semiconductor, together with their natural isotopic abundance in percent and atomic weight are listed. Let us add an element of beryllium: natural abundance of 9 Be ¼ 100%; atomic weight ¼ 9.012182(3).

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

10

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.1 Phillips’s ionicity fi for a number of group-IV, III–V and II–VI semiconductors IV Diamond Si Ge Sn SiC

fi

III–V

fi

II–VI

fi

0 0 0 0 0.177

BN BP BAs AlN AlP AlAs AlSb GaN GaP GaAs GaSb InN InP InAs InSb

0.221 0.032 0.044 0.449 0.307 0.274 0.250 0.500 0.327 0.310 0.261 0.578 0.421 0.357 0.321

BeO BeS BeSe BeTe MgO MgS MgSe MgTe ZnO ZnS ZnSe ZnTe CdO CdS CdSe CdTe HgS HgSe HgTe

0.602 0.286 0.261 0.169 0.841 0.786 0.790 0.554 0.616 0.623 0.630 0.609 0.785 0.685 0.699 0.717 0.790 0.680 0.650

The molecular weight M for an ANB8N compound semiconductor (N„ 4) can be simply given by the sum of the atomic weights of atoms A and B. For an elemental semiconductor (N ¼ 4), it is given by the atomic weight of the element atom A ¼ B. The molecular weight M of any alloy semiconductors can be obtained from the linear interpolation scheme. 0.25 CxSi1-x

fi

0.20

(a)

SiC

0.15 Ordered alloy

0.10 0.05 0

0

0.2

0.4

1.0

x

0.6

0.8

1.0

Mgx Zn1-x SySe1-y /GaAs (x)

0.8 fi

Disordered alloy

0.6 Gax In1-x Py As1-y /InP (y)

0.4 0.2 0

AlxGa1-x As

(b) 0

0.2

0.4

0.6 x or y

0.8

1.0

Figure 1.1 Phillips ionicity fi versus x or y for (a) CxSi1x and (b) AlxGa1xAs, GaxIn1xPyAs1y/InP and MgxZn1xSySe1y/GaAs. The open and solid circles in (a) show the endpoint and SiC (x ¼ 0.5) values, respectively. The solid lines in (b) are calculated from Equation (1.1)

STRUCTURAL PROPERTIES

11

1.3 CRYSTAL STRUCTURE 1.3.1 Random Alloy Table 1.2 summarizes the crystal classes for easily obtained or normally grown: (a) group-IV elemental semiconductors, (b) III–V and (c) II–VI binary semiconductors. In Table 1.2(a), the crystal classes for an easily grown compound semiconductor SiC are also included. Table 1.2 Summary of crystal structure for: (a) group-IV, (b) III–V and (c) II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite (C6v); h ¼ hexagonal (C6v or D6h); rh ¼ rhombohedral; t ¼ tetragonal; rs ¼ rocksalt; or ¼ orthorhombic. Note that b-Sn (t) is a metal (a) IV

C

Si

C Si Ge Sn

d zb, w, h, rh

zb, w, h, rh d

Ge

d

Sn

d, t

(b) III/V

N

P

As

Sb

B Al Ga In

zb, h w w w

zb zb zb zb

zb zb zb zb

zb zb zb

(c) II/VI

O

S

Se

Te

Be Mg Zn Cd Hg

w rs w rs rh, or

zb rs zb, w w zb, rh

zb zb zb w zb

zb w zb zb zb

1.3.2 Spontaneous Ordering (a) Group-IV semiconductor alloy The phenomenon of spontaneous ordering in semiconductor alloys is observed to occur spontaneously during epitaxial growth of certain semiconductor alloys and results in a modification of their structural, electronic and optical properties [2]. Substantial effort has been focused on learning how to control this phenomenon so that it may be used for tailoring desirable material properties. We summarize in Table 1.3 the spontaneous ordering phases observed in some group-IV, III–V and II–VI semiconductor alloys.

12

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.3 Types of spontaneous ordering phases observed in some group-IV, III–V and II–VI semiconductor alloys System

Ordering type

Material

Epitaxial growth

IV

RS1 (CuPt) RS2 (CuPt) RS3 (CuPt)

SiGe SiGe SiGe

MBEa MBEa MBEa

III–V

CuPt-B

AlInP GaInP AlInAs GaInAs GaInSb GaPAs GaPSb GaAsSb InPAs InPSb InAsSb GaInPAs AlGaInP AlInP AlInAs AlGaAs GaInAs GaAsSb AlInAs GaInAs

MBE,b MOCVDc Cl-VPE,d HT-VPE,e MBE,f MOCVDg MEB,h MOCVDi Cl-VPE,j MOCVDk MOCVDl MOCVDm MOCVDn MBEo MOCVDp MOCVDq MOCVD,r MBEs Cl-VPE,j MOCVDt MOCVDc MBEb MBEu MOCVDv MBEw MBE,x MOCVDy MBEz MBEaa

ZnCdTe CdHgTe ZnSeTe ZnCdTe ZnSeTe ZnCdTe

MOCVDab LPEac MOCVDad MBEae MBEaf MBEag

CuPt-A CuAu-I TP-A

II–VI

CuPt-B CuAu-I Cu3Au

See, W. J€ager, in Properties of Strained and Relaxed Silicon Germanium, EMIS Datareviews Series No. 12 (edited by E. Kasper), INSPEC, London, 1995, p. 53 b A. Gomyo et al., Jpn. J. Appl. Phys. 34, L469 (1995) c T. Suzuki et al., Jpn. J. Appl. Phys. 27, 2098 (1988) d O. Ueta et al., J. Appl. Phys. 68, 4268 (1990) e K. Nishi and T. Suzuki (unpublished) f A. Gomyo et al., Mater. Res. Symp. Proc. 417, 91 (1996) g A. Gomyo et al., Phys. Rev. Lett. 60, 2645 (1988) h T. Suzuki et al., Appl. Phys. Lett. 73, 2588 (1998) i A. G. Norman et al., Inst. Phys. Conf. Ser. 87, 77 (1987) j M. A. Shahid et al., Phys. Rev. Lett. 58, 2567 (1987) k T.-Y. Seong et al., J. Appl. Phys. 75, 7852 (1994) l J. Shin et al., J. Electron. Mater. 24, 1563 (1995) m G. S. Chen et al., Appl. Phys. Lett. 57, 2475 (1990) n G. B. Stringfellow, J. Cryst. Growth 98, 108 (1989) a

STRUCTURAL PROPERTIES

13

Figure 1.2 Si–Ge ordered structures of types (a) RS1, (b) RS2 and (c) RS3. In (c), the four projected compositions a, b, g and d correspond to specific Si- and Ge-rich sites

Normally, SixGe1x crystallizes in the diamond structure which contains of two fcc sublattices shifted by one quarter of the body diagonal. Observations of long-range ordering of group-IV semiconductor alloy have been made on SixGe1x layers grown on Si(100) by MEB [3] and subsequently at interfaces of SLs [2]. Different order structures were suggested in bulk SixGe1x on the basis of experimental results and are depicted in Figure 1.2. They are RS1, RS2 and RS3 with the rhombohedral structures (CuPt ordering, R3m). The stoichiometry for RS1 and RS2 is Si0.5Ge0.5, while RS3 allows compositional differences on specific lattice sites. As seen in Figure 1.2, RS1 (RS2) has the widely (closely) spaced {111} planes occupied by the same atom type, while RS3 allows compositional differences between projected sites or columns with compositions a, b, g and d corresponding to specific Si- and Ge-rich sites.

3 Y.-E. Ihm et al., Appl. Phys. Lett. 51, 2013 (1987) D. H. Jaw et al., Appl. Phys. Lett. 59, 114 (1991) q See, H. R. Jen et al., Appl. Phys. Lett. 54, 1890 (1989) r H. R. Jen et al., Appl. Phys. Lett. 54, 1154 (1989) s T.-Y. Seong et al., Appl. Phys. Lett. 64, 3593 (1994) t W. E. Plano et al., Appl. Phys. Lett. 53, 2537 (1988) u T. Suzuki et al., Appl. Phys. Lett. 73, 2588 (1998) v T. S. Kuan et al., Phys. Rev. Lett. 54, 201 (1985) w O. Ueda, et. al., J. Cryst. Growth 115, 375 (1991) x O. Ueta et al., Proc. 7th Int. Conf. InP and Related Materials Sapporo, Japan, p. 253 (1995) y H. R. Jen et al., Appl. Phys. Lett. 48, 1603 (1986) z A. Gomyo et al., Phys. Rev. Lett. 72, 673 (1994) aa D. Shindo et al., J. Electron Microscopy 45, 99 (1996) ab N. Amir et al., J. Phys. D: Appl. Phys. 33, L9 (2000) ac K. T. Chang and E. Goo, J. Vac. Sci. Technol. B 10, 1549 (1992) ad K. Wolf et al., Solid State Commun. 94, 103 (1995) ae H. S. Lee et al., Appl. Phys. Lett. 83, 896 (2003) af H. Luo et al., J. Vac. Sci. Technol. B 12, 1140 (1994) ag H. S. Lee et al., Solid State Commun. 137, 70 (2006) o p

14

PROPERTIES OF SEMICONDUCTOR ALLOYS

The long-range order parameter in RS1 and RS2 can be defined by rSi x S¼ 1x

ð1:2Þ

where rSi is the fraction of Si sites occupied correctly and x is the fraction of Si atoms in SixGe1x. S ¼ 1 means perfect and complete order, while S ¼ 0 means random alloy. The degree of long-range order can be quantitatively deduced from the electron diffraction intensity of superstructure reflections. However, because of the presence of crystalline defects, of superposition of various domains and of the multiple scattering, the actual intensity substantially deviates from the kinematic value so that quantitative determination from selected-area electron diffraction intensity is usually obscured [2]. Observations of the long-range ordering have been made on bulk SiGe or SL samples prepared by MBE at medium temperature and for various compositions. However, no observations of ordered phases are reported for bulk SiGe grown from the melt [4]. (b) III–V semiconductor alloy In 1985, Kuan et al. [5] first observed an ordered phase (CuAu-I type) in III–V semiconductor alloy which was an AlGaAs epilayer grown on GaAs(100) at 600–800 C by MOCVD. Since the finding of CuPt-type ordering in SiGe alloy [3], this type of ordering (CuPt-B) has also been reported for many III–V alloys, such as AlInP, GaInP, AlInAs and GaInAs ([6], see also Table 1.3). New types of ordering, CuPt-A and TP-A, are also found in AlInP [7] and AlInAs alloys [8]. Other types of ordering, CuAu-I, famatinite and chalcopyrite, are reported in the early history of the spontaneous ordering in III–Valloys; however, mechanism of these phases seems to be quite different from those of CuPt-B, CuPt-A and TP-A [6]. The unit cells of (a) CuPt-B, (b) CuAu-I and (c) chalcopyrite structures are shown in Figure 1.3. The metallurgical CuPt alloy has a random fcc structure at high temperatures, but quenching at low temperatures produces a rhombohedral phase with 1/2{111} chemical ordering. The CuPt-B structure is among the most widely discussed and accessed forms of spontaneous ordering in III–V ternaries, and occurs in both common anion and common cation alloys (Table 1.3). It is a monolayer SL of IIIA (VA)-rich planes and IIIB (VB)-rich planes ordered in the ½ 111 or ½1 11 directions, as depicted in Figure 1.4. The CuPt-A and

Figure 1.3 Unit cells of (a) CuPt-B (GaInAs), (b) CuAu-I (AlGaAs) and (c) chalcopyrite structures (CuGaSe2)

STRUCTURAL PROPERTIES

15

Figure 1.4 [110] projection of CuPt-B ordering (GaInP)

1 1 and ½111 directions, in which CuPt-B ordering is never TP-A phases occur in the ½1 observed. The metallic CuAu alloy shows two prominent ordered phases: (i) CuAu-I trigonal phase with alternating (002) planes of pure Cu and Au compositions and (ii) orthorhombic CuAu-II phase. The CuAu-I ordering occurs spontaneously within fcc sublattices of some III–V pseudobinary alloys, such as AlGaAs, GaInAs and GaAsSb (Table 1.3). An earlier thermodynamic calculation based on a first-principles theory predicted that an ordered phase with a large lattice-constant mismatch is more stable than the corresponding random phase [9]. Some experimental data, on the other hand, showed that the kinetics of crystal growth plays an important role in the formation of an ordered structure as discussed in Mascarenhas [2]. (c) II–VI semiconductor alloy Only a few studies have been carried out on spontaneous ordering of II–VI semiconductor alloys. These studies reported ordering of CuPt and CuAu-I types (Table 1.3). Recently, a new ordering phase, Cu3Au, has been observed in Zn0.9Cd0.1Te epilayers grown on GaAs(100) substrates [10]. We can see a tendency in Table 1.3 to observe the CuPt (CuAu-I) phase if samples were grown by MOCVD (MBE).

1.4 LATTICE CONSTANT AND RELATED PARAMETERS 1.4.1 CuAu Alloy: Ordered and Disordered States Cu–Au alloy is among the best studied of all metallic alloys. The most interesting feature of this alloy is that CuAu (x ¼ 0.5), CuAu3 (x ¼ 0.25) and Cu3Au (x ¼ 0.75) can be obtained in either ordered or disordered form. The ordered CuAu alloy crystallizes in the LI0 tetragonal structure

16

PROPERTIES OF SEMICONDUCTOR ALLOYS 5.0 Cux Au1-x

a (Å)

4.5 4.0 3.5

CuAu3 (LI2) Cu3Au (LI2)

3.0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.5 Lattice constant a versus x for CuxAu1x. The solid and open circles represent the ordered (x ¼ 0.25, 0.75) and disordered alloy values, respectively. The solid line shows the linear interpolation result between the endpoint elemental data

(space group ¼ P4/mmm), while the ordered CuAu3 and Cu3Au alloys crystallize in the LI2 cubic structure ðPm 3mÞ. In Figure 1.5 the lattice constant a has been plotted as a function of x for CuxAu1x. The solid and open circles represent the ordered and disordered alloy data, respectively. The solid line shows the linear interpolation result between the Au (x ¼ 0) and Cu (x ¼ 1.0) values. It can be seen from Figure 1.5 that the Cu–Au ordering has no strong effect on the lattice parameter. Similarly, no clear spontaneous ordering effect has been observed on the lattice parameters of semiconductor alloys.

1.4.2 Non-alloyed Semiconductor The lattice parameters for a number of the most easily grown group-IV, III–V and II–VI semiconductors are listed in Table 1.4. Tables 1.5, 1.6 and 1.7 also list the molecular weight (M), lattice constants (a and b) and crystal density (g) for a number of group-VI, III–Vand II–VI semiconductors crystallizing in the diamond, zinc-blende and wurtzite structures, respectively. These values can be used to obtain alloy values using the interpolation scheme.

Table 1.4 Most easily grown crystal structure and lattice constants at 300 K for a number of easily or normally grown group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; h ¼ hexagonal; w ¼ wurtzite; rs ¼ rocksalt; or ¼ orthorhombic; rh ¼ rhombohedral

System

Material

Crystal structure

a (A)

c (A)

IV

Diamond Si Ge Sn 3C-SiC 6H-SiC

d d d d zb h

3.5670 5.4310 5.6579 6.4892 4.3596 3.0806

15.1173

System

Material

Crystal structure

a (A)

c (A)

STRUCTURAL PROPERTIES

17

Table 1.4 (Continued )

System

Material

Crystal structure

a (A)

III–V

BN BN BP BAs AlN AlP AlAs AlSb GaN GaP GaAs GaSb InN InP InAs InSb

zb h zb zb h (w) zb zb zb h (w) zb zb zb h (w) zb zb zb

3.6155 2.5040 4.5383 4.777 3.112 5.4635 5.66139 6.1355 3.1896 5.4508 5.65330 6.09593 3.548 5.8690 6.0583 6.47937

BeO BeS BeSe BeTe MgO MgS MgSe MgTe ZnO ZnS ZnS ZnSe ZnTe CdO CdS CdSe CdTe HgO

h (w) zb zb zb rs rs zb h (w) h (w) h (w) zb zb zb rs h (w) h (w) zb or

HgS

rh

HgSe HgTe

zb zb

2.6979 4.865 5.137 5.617 4.203 5.203 5.91 4.548 3.2495 3.8226 5.4102 5.6692 6.1037 4.686 4.1367 4.2999 6.481 3.577 (a) 8.681 (b) 2.427 (c) 0.745 (u) 4.14 (a) 9.49 (b) 2.292 (c) 0.720 (u) 0.480 (v) 6.084 6.4603

II–VI

c (A) 6.6612 4.982

5.1855

5.760

4.380

7.390 5.2069 6.2605

6.7161 7.0109

Table 1.5 Molecular weight M, lattice constant a and crystal density g for a number of cubic, diamondtype semiconductors at 300 K System

Material

M (amu)

a (A)

g (g/cm3)

IV

Diamond Si Ge Sn

12.0107 28.0855 72.61 118.710

3.5670 5.4310 5.6579 6.4892

3.5156 2.3291 5.3256 5.7710

Table 1.6 Molecular weight M, lattice constant a and crystal density g for a number of cubic, zincblende-type semiconductors at 300 K g (g/cm3)

40.0962

4.3596

3.2142

BN BP BAs AlN AlP AlAs AlSb GaN GaP GaAs GaSb InN InP InAs InSb

24.818 41.785 85.733 40.98828 57.955299 101.903098 148.742 83.730 100.696 144.645 191.483 128.825 145.792 189.740 236.578

3.6155 4.5383 4.777 4.38 5.4635 5.66139 6.1355 4.52 5.4508 5.65330 6.09593 4.986 5.8690 6.0583 6.47937

3.4880 2.9693 5.224 3.24 2.3604 3.73016 4.2775 6.02 4.1299 5.31749 5.61461 6.903 4.7902 5.6678 5.77677

BeO BeS BeSe BeTe MgO MgS MgSe MgTe ZnO ZnS ZnSe ZnTe CdO CdS CdSe CdTe HgS HgSe HgTe

25.0116 41.078 87.97 136.61 40.3044 56.371 103.27 151.91 81.39 97.46 144.35 192.99 128.410 144.477 191.37 240.01 232.66 279.55 328.19

3.80 4.865 5.137 5.617 4.21 5.62 5.91 6.42 4.47 5.4102 5.6692 6.1037 5.148a 5.825 6.077 6.481 5.8514 6.084 6.4603

3.03 2.370 4.310 5.120 3.59 2.11 3.32 3.81 6.05 4.0879 5.2621 5.6372 6.252a 4.855 5.664 5.856 7.7135 8.245 8.0849

Material

IV

3C-SiC

III–V

II–VI

a

Theoretical

a (A)

System

M (amu)

STRUCTURAL PROPERTIES

19

Table 1.7 Molecular weight M, lattice constants a and c and crystal density g for a number of hexagonal, wurtzite-type semiconductors at 300 K System

Material

a IV

2H-SiC

III–V

II–VI

a

g (g/cm3)

Lattice constant (A)

M (amu)

c

40.0962

3.0763

5.0480

3.2187

AlN GaN InN

40.98828 83.730 128.825

3.112 3.1896 3.548

4.982 5.1855 5.760

3.258 6.0865 6.813

BeO BeSa BeSea BeTea MgO MgS MgSe MgTe ZnO ZnS ZnSe ZnTe CdO a CdS CdSe CdTe HgS a HgSe a HgTe a

25.0116 41.078 87.97 136.61 40.3044 56.371 103.27 151.91 81.39 97.46 144.35 192.99 128.410 144.477 191.37 240.01 232.66 279.55 328.19

2.6979 3.440 3.632 3.972 3.199 3.972 4.145 4.548 3.2495 3.8226 3.996 4.27 3.678 4.1367 4.2999 4.57 4.1376 4.302 4.5681

4.380 5.618 5.932 6.486 5.086 6.443 6.723 7.390 5.2069 6.2605 6.626 6.99 5.825 6.7161 7.0109 7.47 6.7566 7.025 7.4597

3.009 2.370 4.311 5.120 2.970 2.127 3.429 3.811 5.6768 4.0855 5.232 5.81 6.249 4.8208 5.6615 5.90 7.7134 8.246 8.0850

Estimated or theoretical

1.4.3 Semiconductor Alloy (a) Group-IV semiconductor Table 1.8 gives the lattice-matching condition between some group-IV ternary alloys and Si substrate. The incorporation of carbon into Si or SiGe gives rise to additional flexibility for group-IV-based heterostructure design [11]. Due to huge lattice mismatch between diamond Table 1.8 Lattice-matching conditions of some group-IV ternaries at 300 K Material

Substrate

Expression

Remark

CxSiyGe1xy CxSiySn1xy CxGeySn1xy

Si Si Si

x ¼ 0.109–0.109y x ¼ 0.362–0.362y x ¼ 0.362–0.284y

0 y 1.0, x/(1 x y) ¼ 0.122 0 y 1.0, x/(1 x y) ¼ 0.567 0 y 0.89

20

PROPERTIES OF SEMICONDUCTOR ALLOYS

and Si, a small amount of substantially incorporated C induces a substantial tensile strain in pseudomorphic CxSi1x layers on Si. This effect can be exploited for CxSiyGe1xy/Si, CxSiySn1xy/Si and CxGeySn1xy/Si heterostructures by properly choosing pseudomorphic compositions x and y. It should be noted, however, that the solubility of C into Si is only about 6 106 at% (3 1017 cm3) at the melting point of Si. Carbon incorporated into substitutional lattice sites up to a few atomic percent has been achieved only using growth techniques far from thermodynamic equilibrium [12]. Figure 1.6 shows the plot of the lattice constant a versus x for bulk CxSi1x. The open circles represent the experimental data for diamond and Si, while the solid circle shows the data for 6.0

a (Å)

5.5

CxSi1-x

5.0 4.5 4.0 3C-SiC

3.5 3.0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.6 Lattice constant a versus x for bulk CxSi1x at 300 K. The open and solid circles represent the experimental data. The light solid and dashed lines represent the results of Vegard law between Si (x ¼ 0) and 3C-SiC (x ¼ 0.5) and between Si (x ¼ 0) and diamond (x ¼ 1.0), respectively. The heavy solid line shows the theoretical values obtained from a Monte Carlo simulation by Kelires [13]

3C-SiC (x ¼ 0.5). The light solid line is obtained from Vegard law between Si and 3C-SiC (x ¼ 0.5), while the dashed line is obtained between Si and diamond (x ¼ 1.0). The 3C-SiC value is smaller than the linearly interpolated value. The heavy solid line in Figure 1.6 represents the theoretical a values for C xSi1x obtained from a Monte Carlo calculation [13]. These values can be expressed as (in A) aðxÞ ¼ 5:43102:4239x þ 0:5705x2

ð1:3Þ

The negative deviation a(x) seen in Figure 1.6 has been confirmed experimentally from pseudomorphic CxSi1x epilayers (x < 0.012) grown on Si(100) by solid-source MBE [14]. Si and Ge, both crystallize in the diamond structure, form a continuous series of SixGe1x alloys with x ranging from 0 to 1.0. The most precise and comprehensive determination of the lattice constant a and crystal density g across the whole alloy range was undertaken by Dismukes et al. [15]. The values they obtained for a and g are plotted versus x for SixGe1x in Figure 1.7. These data reveal a small deviation from Vegard law, i.e. from the linearity between the endpoint values. The lattice parameter a shows a downward bowing, while the density parameter g gives an upward bowing. From Figure 1.7, we obtain parabolic relation for a and g as a function of x (a in A, g in g/cm3) aðxÞ ¼ 5:65750:2530x þ 0:0266x2

ð1:4aÞ

gðxÞ ¼ 5:32562:5083x0:4853x2

ð1:4bÞ

STRUCTURAL PROPERTIES

21

5.7 a (Å)

(a) 5.6 5.5

SixGe1-x

g (g/cm3)

5.4 6 (b)

5 4 3 2

0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.7 (a) Lattice constant a and (b) crystal density g for SixGe1x at 300 K. The experimental data are taken from Dismukes et al. [15]. The solid and dashed lines represent the parabolic and linear fit results, respectively

As shown in Figure 1.8, the diamond-type lattice, e.g. Si has only one type of first-neighbor distance pﬃﬃﬃ 3 a ðfour bondsÞ ð1:5Þ dðSiSiÞ ¼ 4 EXAFS has been popularly used to determine bond lengths for different types of neighbor atom pairs and the corresponding fractional occupancy of each type of neighbor. Recent EXAFS and XRD studies performed on strained SixGe1x/Si layers indicated that the Si–Si, Si–Ge and Ge–Ge nearest-neighbor distances are 2.35 0.02, 2.42 0.02 and 2.38 0.02 A, respectively, close to the sum of their constituent-element covalent radii and independent of x, while the lattice constant varies monotonically with x [16,17]. More recently, Yonenaga et al. [18] investigated the local atomistic structure in bulk Czochralski-grown SixGe1x using EXAFS. As shown in Figure 1.9, the bond lengths Si–Si, Si–Ge and Ge–Ge in the bulk SixGe1x remain distinctly different lengths and vary in linear fashion of x over the entire composition range 0 x 1.0, in agreement with expectation derived from ab-initio electronic structure calculation. These results suggest that SixGe1x is a typical disorder material and that the bond lengths and bond angles are disordered with x in SixGe1x.

Figure 1.8 Bond distances in (a) diamond (Si), (b) zinc-blende (GaAs) and (c) wurtzite structures (GaN)

22

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 1.9 Near-neighbor distance in SixGe1x at 300 K. The experimental data are taken from Yonenaga et al. [18]. The horizontal lines show the bond lengths in bulk Si and Ge. The middle thin line is obtained from Vegard law

(b) III–V semiconductor The expressions for a versus alloy composition can be obtained from Vegard law. The crystal density can also be calculated from g ¼ MdM/NA, where M is the molecular weight, NA ¼ 6.022 1023 mol1 is the Avogadro constant and dM is the molecular density [1]. The III–V quaternaries can be epitaxially grown on some III–V binaries (GaAs, InP, etc.). Introducing the binary lattice parameters in Table 1.6 into Equation (A.6) or Equation (A.8), we can obtain the lattice-matching conditions for AxB1xCyD1y and AxByC1xyD quaternaries on various III–V binary substrates. These results are summarized in Tables 1.9–1.11. The lattice-matching conditions in Tables 1.9–1.11 can be approximated by more simple expressions. Some results are presented in Table 1.12. The lattice parameter a at 300 K as a function of x for AlxGa1xAs is shown in Figure 1.10. The experimental data are taken from Takahashi [19]. From a least-squares fit, we obtain aðxÞ ¼ 5:6533 þ 0:0083x0:0003x2

ð1:6Þ

The solid line in Figure 1.10 shows the calculated result of Equation (1.6). This equation promises that the lattice parameter for AlxGa1xAs can be given by Vegard law with good Table 1.9 Lattice-matching conditions for some cubic, zinc-blende-type III–V quaternaries of type AxB1xCyD1y at 300 K x¼

A0 þ B0 y C0 þ D0 y

Quaternary

Substrate

A0

B0

C0

D0

AlxIn1xPyAs1y

GaAs InP GaAs InP

0.4050 0.1893 0.4050 0.1893

0.1893 0.1893 0.1893 0.1893

0.3969 0.3969 0.4050 0.4050

0.0086 0.0086 0.0132 0.0132

GaxIn1xPyAs1y

Remark 0.04y1.0 0y1.0 0y1.0 0y1.0

STRUCTURAL PROPERTIES

23

Table 1.10 Lattice-matching conditions for some cubic, zinc-blende-type III–V quaternaries of type AxB1xCyD1y at 300 K y¼

A0 þ B0 x C0 þ D0 x

Quaternary

Substrate

A0

B0

C0

D0

AlxGa1xPyAs1y AlxGa1xPySb1y

GaAs GaAs GaSb InP InAs GaSb InP InAs GaAs GaSb InP InAs GaSb InP InAs GaAs GaSb InP InAs GaSb InP InAs

0 0.4426 0 0.2269 0.0376 0 0.2269 0.0376 0.8261 0.3834 0.6104 0.4211 0.3834 0.6104 0.4211 0.8261 0.3834 0.6104 0.4211 0.3834 0.6104 0.4211

0.0081 0.0396 0.0396 0.0396 0.0396 0.0396 0.0396 0.0396 0.3439 0.3439 0.3439 0.3439 0.3439 0.3439 0.3439 0.3834 0.3834 0.3834 0.3834 0.3834 0.3834 0.3834

0.2025 0.6451 0.6451 0.6451 0.6451 0.4426 0.4426 0.4426 0.6104 0.6104 0.6104 0.6104 0.4211 0.4211 0.4211 0.6104 0.6104 0.6104 0.6104 0.4211 0.4211 0.4211

0.0046 0.0269 0.0269 0.0269 0.0269 0.0315 0.0315 0.0315 0.0616 0.0616 0.0616 0.0616 0.0530 0.0530 0.0530 0.0348 0.0348 0.0348 0.0348 0.0216 0.0216 0.0216

AlxGa1xAsySb1y AlxIn1xPySb1y

AlxIn1xAsySb1y GaxIn1xPySb1y

GaxIn1xAsySb1y

Remark 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0.53 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0.48 x 1.0 0 x 1.0 0.52 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0.47 x 1.0 0 x 1.0

Table 1.11 Lattice-matching conditions for some cubic, zinc-blende-type III–V quaternaries of the type AxByC1xyD or ABxCyD1xy at 300 K Quaternary

Substrate

Expression

Remark

AlxGayIn1xyP AlxGayIn1xyAs AlPxAsySb1xy

GaAs InP GaAs InP InAs GaAs InP InAs GaSb InAs

y ¼ 0.5158–0.9696x y ¼ 0.4674–0.9800x x ¼ 0.7176–0.7055y x ¼ 0.3966–0.7055y x ¼ 0.1149–0.7055y x ¼ 0.6861–0.6861y x ¼ 0.3518–0.6861y x ¼ 0.0583–0.6861y x ¼ 0.6282–0.6899y x ¼ 0.6899–0.6899y

0 x 0.53 0 x 0.48 0 y 1.0 0 y 0.56 0 y 0.16 0 y 1.0 0 y 0.51 0 y 0.08 0 y 0.91 0 y 1.0

GaPxAsySb1xy InPxAsySb1xy

24

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.12 Approximated lattice-matching expression for some important cubic, zinc-blende-type III–V quaternaries at 300 K Quaternary

Substrate

Expression

Remark

AlxGa1xAsySb1y

GaSb InAs InP GaSb InAs GaAs InP

y ¼ 0.084x y ¼ 0.085 þ 0.078x x ¼ 0.47–0.47y y ¼ 0.91–0.91x y ¼ 1.00–0.91x y ¼ 0.52–0.97x y ¼ 0.47–0.98x

0 x 1.0 0 x 1.0 0 y 1.0 0 x 1.0 0 x 1.0 0 x 0.53 0 x 0.48

GaxIn1xPyAs1y GaxIn1xAsySb1y AlxGayIn1xyP AlxGayIn1xyAs

5.665 AlxGa1-xAs a (Å)

5.660

5.655

5.650 0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.10 Lattice parameter a as a function of x for AlxGa1xAs at 300 K. The experimental data are taken from Takahashi [19]. The solid line represents the quadratic least-squares fit

approximation. The difference in a between AlxGa1xAs and GaAs can also be written as aðAlx Ga1x AsÞaðGaAsÞ ¼ 0:0015x ¼ 0:15x% aðGaAsÞ

ð1:7Þ

Figure 1.11 shows the experimental x–y plots for GaxIn1xPyAs1y/InP [20]. The solid line shows the exactly calculated x–y relation in Table 1.9 1.0 Ga x In1-xPyAs1-y /InP

0.8 y

0.6 0.4 Exact Approx.

0.2 0

0

0.1

0.2

0.3

0.4

0.5

x

Figure 1.11 Plots of x versus y for GaxIn1xPyAs1y nearly lattice-matched to InP at 300 K. The experimental data are taken from Nahory et al. [20]. The solid and dashed lines show the lattice-matching relationships obtained from Vegard law in Equations (1.8) and (1.9), respectively

STRUCTURAL PROPERTIES

x¼

0:18930:1893y 0:4050 þ 0:0132y

25

ð1:8Þ

The dashed line also shows the calculated result using an expression in Table 1.12 x ¼ 0:470:47y

ð1:9Þ

Both expressions can explain the experimental x–y relation very well and simultaneously indicate the validity of Vegard law for GaxIn1xPyAs1y/InP. It has, however, been reported that strained AlxGa1xSb/GaSb does not obey Vegard law [21]. The crystal density g versus y for GaxIn1xPyAs1y/InP is shown in Figure 1.12. The solid line represents the X-ray crystal density calculated from Equation (1.16) of Adachi [1], while the dashed line is obtained from the linear interpolation between the endpoint densities (y ¼ 0, 1.0). Their difference is within 2%. 6.0 GaxIn1-xPyAs1-y/InP

g (g/cm-3)

5.5 5.0

Exact Approx.

4.5 4.0 0

0.2

0.4

0.6

0.8

1.0

y

Figure 1.12 X-ray crystal density g versus y for GaxIn1xPyAs1y/InP at 300 K. The solid line represents the exact X-ray crystal density calculated from Equation (1.16) of Adachi [1], while the dashed line is obtained from the linear interpolation between the endpoint binary data

The experimental lattice parameter c as a function of x for w-GaxIn1xN is plotted in Figure 1.13. The experimental data are taken from Bearch et al. [22] (solid circles) and Romano et al. [23] (open circles). The GaxIn1xN layers (0 x 0.14) used by Bearch et al. [22] were grown on (0001) sapphire by MOMBE and were believed to be fully relaxed. On the other hand, the GaxIn1xN layers in Romano et al. [23] were pseudomorphically grown on 5 mm thick GaN on (0001) sapphire by MOCVD (x ¼ 0–0.114). The solid line in Figure 1.13 obeys Vegard law using c ¼ 5.1855 A for GaN and c ¼ 5.760 A for InN (Table 1.7). Figure 1.14 shows the lattice parameter c versus x for strained AlxGa0.9xIn0.1N alloy grown by MOCVD [24]. The dashed line represents the linear interpolation result using the endpoint values taken from Table 1.7. The lattice parameter c is found to decrease almost linearly with increasing x. The prediction of Vegard law gives no good agreement with the experimental data. It can be concluded from Figure 1.13 that the fully relaxed GaxIn1xN films follow Vegard law well; however, no good agreement can be achieved in the case of the pseudomorphic alloy layers. As we will see later (Section 1.5.2), Vegard law may be applicable if any strain effects are artificially removed from such pseudomorphically strained layers. HRXRD has been widely used and demonstrated that almost all III–V semiconductor alloys obey Vegard law well. It has also been reported that Vegard law remains valid in dilute nitrides, such as GaNxAs1x and GaxIn1xNyAs1y, as long as all N atoms in the dilute nitrides locate at the arsenic sites [25]. The N–N pairs are thought to be the predominant N-related defects that cause deviation from Vegard law [26]. Germini et al. [21], however, observed a deviation

26

PROPERTIES OF SEMICONDUCTOR ALLOYS 5.30

c (Å)

5.28

w-GaxIn1-xN

5.26 5.24 5.22 5.20 5.18 0.80

Vegard law

0.85

0.90 x

0.95

1.00

Figure 1.13 Lattice parameter c as a function of x for w-GaxIn1xN at 300 K. The experimental data are taken from Bearch et al. [22] (fully relaxed layers, solid circles) and Romano et al. [23] (pseudomorphic layers, open circles). The solid line represents the simply estimate of the c versus x relationship obtained from Vegard law 5.30

c (Å)

5.25

w-AlxGa0.9-xIn0.1N

5.20 5.15 5.10 0

Vegard law

0.05 0.10 0.15 0.20 0.25 0.30 x

Figure 1.14 Lattice parameter c versus x for strained w-AlxGa0.9xIn0.1N at 300 K. The experimental data are taken from Aumer et al. [24]. The dashed and solid lines represent the results of applying Vegard law before and after correcting for the biaxial strain effect

from Vegard law in MBE-grown AlxGa1xSb/GaSb layers by HRXRD, RBS and RHEED. These results are plotted in Figure 1.15. The experimental unstrained lattice parameters can be described by aðxÞ ¼ 6:09593 þ 0:04360x4:229 103 x2

ð1:10Þ

The deviation from linearity is found to be larger than the prediction of a perfect random alloy in the frame of the Fournet model [27]. There is a significant structural difference between the bond distance in the zinc-blende and wurtzite structures of AxB1xC alloy. The first-neighbor distance in the zinc-blende structure is given from Figure 1.8 by pﬃﬃﬃ 3 dðGaAsÞ ¼ a ðfour bondsÞ ð1:11Þ 4 Yet, the wurtzite structure has two types of the first-neighbor anion–cation bond distances (Figure 1.8) dðGaN1 Þ ¼ ua ðone bondÞ

ð1:12aÞ

STRUCTURAL PROPERTIES

27

6.140 Al xGa 1-x Sb

a (Å )

6.130 6.120 6.110 6.100 6.090

0

0. 2

0. 4

0. 6

0. 8

1. 0

x

Figure 1.15 Room-temperature lattice constant a as a function of x for AlxGa1xSb grown on GaSb. The experimental data are taken from Germini et al. [21]. The solid line represents the quadratic best-fit result obtained using Equation (1.10)

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 1 1 c þ u aw ðthree bondsÞ dðGaN2 Þ ¼ 3 2 aw

ð1:12bÞ

where u represents the cell-internal structural parameter and aw and c show the lengths of the lattice vectors of the wurtzite structure. In the case of an ideal tetragonal ratio c/aw ¼ (8/3)1/2 ¼ 1.6330 and an ideal cell internal parameter u ¼ 3/8, it follows from Equation (1.12) that d(Ga–N1) ¼ d(Ga–N2). In the zinc-blende lattice, we have only one type of second neighbor cation–anion bond distance pﬃﬃﬃﬃﬃ 11 a ð12 bondsÞ ð1:13Þ dðGaAsÞ ¼ 4 On the other hand, the wurtzite lattice has three types of second neighbor cation–anion distances concerning the cation A (Ga) to anions C2a, C2b and C2c c dðGaN2a Þ ¼ ð1uÞ aw ðone bondÞ ð1:14aÞ aw sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 uc aw ðsix bondsÞ dðGaN2b Þ ¼ 1 þ ð1:14bÞ aw sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 4 1 c þ u aw ðthree bondsÞ ð1:14cÞ dðGaN2c Þ ¼ 3 2 aw For ideal wurtzite parameters of c/aw ¼ (8/3)1/2 ¼ 1.6330 and u ¼ 3/8, the following expression can be obtained from Equation (1.14) dðGaN2a Þ ¼ 1:0206aw ; dðGaN2b Þ ¼ dðGaN2c Þ ¼ 1:1726aw

ð1:15Þ

The spacing between the near-neighbor In–In or P–P atoms in InP is equal to (1/H2)a. It would be anticipated that for an alloy the interatomic bond length of each constituent remains constant with alloy composition. Unfortunately, however, standard XRD techniques give information only on the lattice structure that is averaged over an area larger than the scale of

28

PROPERTIES OF SEMICONDUCTOR ALLOYS

lattice constant. The interatomic structure in such semiconductor alloys was, therefore, not well understood until 1982. Mikkelsen and Boyce [28] reported in 1982 the interatomic structure of GaxIn1x As using an EXAFS. They found that the Ga–As and In–As near-neighbor distances change by only 0.04 A as the In composition varies from 1 to 99 at% despite the fact that this alloy accurately follows Vegard law with a change in average near-neighbor spacing of 0.17 A. We reproduce in Figure 1.16 the results of Mikkelsen and Boyce [28]. They also observed that the cation sublattice approaches a virtual crystal (i.e. an average fcc lattice) with a broadened single distribution of second-neighbor distances, whereas the anion sublattice exhibits a bimodal anion–anion second-neighbor distribution.

Figure 1.16 Near-neighbor distance in GaxIn1xAs at 300 K. The middle thin line represents the bond length curve estimated from Vegard law. [Reprinted with permission from J. C. Mikkelsen, Jr. and J. B. Boyce, Phys. Rev. Lett. 49, 1412 (1982). Copyright (1982) by the American Physical Society]

The essentially same EXAFS results, but on GaxIn1xPyAs1y/InP, were reported by Oyanagi et al. [29]. They reported that the cation–anion distances in GaxIn1xPyAs1y/InP deviate from the average interatomic distance, but are rather close to the bond lengths in pure parent crystals. The cation–anion distances obtained from this study are plotted in Figure 1.17. The near-neighbor distances in w-GaxIn1xN versus x are shown in Figure 1.18. The experimental data are taken from Jeffe et al. [30]. The theoretical lines are taken from Mattila and Zunger [31] in which the valence force field simulation with large supercells (512–1280 atoms) was used. It has been shown [31] that while the first-neighbor cation–anion bonds for different cations (Ga–N1 and In–N1) retain distinct values in the wurtzite and zinc-blende alloys, the second-neighbor cation–anion bonds Ga–N2 and In–N2 merge into a single bond length. However, the second-neighbor cation–anion bonds for the same cation exhibit a crucial difference between the wurtzite and zinc-blende structures. This is thought to be an intrinsic property of the binary constituents and persists in the alloy. The small splitting of the firstneighbor cation–anion bonds in the wurtzite structure is also preserved in the alloy, but obscured by bond length broadening [31].

STRUCTURAL PROPERTIES

29

Near-neighbor distance (Å)

2.70 2.65 2.60

Gax In1-x Py As1-y /InP In-As

2.55 Vegard law

2.50 2.45

Ga-As

2.40

Ga-P

2.35 2.30 0

0.2

0.4

0.6

0.8

1.0

y

Figure 1.17 Near-neighbor distance in GaxIn1xPyAs1y/InP at 300 K. The experimental data are taken from Oyanagi et al. [29]. The dashed line represents the bond length curve obtained from Vegard law

Figure 1.18 Near-neighbor distances versus x for w-GaxIn1xN. The experimental data were measured at 300 K by Jeffe et al. [30]. The theoretically calculated lines are taken from Mattila and Zunger [31] who used the valence force field simulation with large supercells (512–1280 atoms)

(c) II–VI semiconductor Several II–VI semiconductor quaternaries can be epitaxially grown on III–V binary substrates. The corresponding lattice-matching relationships are shown in Tables 1.13 and 1.14. These relationships can be approximated using more simple expressions, as listed in Table 1.15. Figure 1.19 shows the lattice constant a as a function of x for ZnxCd1xTe. The experimental data were obtained at 300 K using an XRD combined with a WDXS [32]. The combination with WDXS led to an absolute composition error Dx of less than 0.01. These data suggest that Vegard

30

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.13 Lattice-matching conditions for some cubic, zinc-blende-type II–VI quaternaries of the type AxB1xCyD1y at 300 K y¼

A0 þ B0 x C0 þ D0 x

Quaternary

Substrate

A0

B0

C0

D0

Remark

MgxZn1xSySe1y MgxZn1xSeyTe1y

GaAs InP

0.016 0.235

0.241 0.314

0.259 0.435

0.031 0.075

0 x 1.0 0 x 0.84

Table 1.14 Lattice-matching conditions for some cubic, zinc-blende-type II–VI quaternaries of the type AxByC1xyD at 300 K Quaternary

Substrate

Expression

Remark

BexMgyZn1xySe MgxZnyCd1xySe

GaAs InP

x ¼ 0.030 þ 0.453y y ¼ 0.510–0.409x

0 y 0.67 0 x 0.83

Table 1.15 Approximated lattice-matching expression for some important cubic, zinc-blende-type II–VI quaternaries at 300 K Quaternary

Substrate

Expression

Remark

MgxZn1xSySe1y MgxZn1xSeyTe1y BexMgyZn1xySe MgxZnyCd1xySe

GaAs InP GaAs InP

y ¼ 0.08 þ 0.82x y ¼ 0.55 þ 0.54x x ¼ 0.03 þ 0.45y y ¼ 0.51–0.41x

0 x 1.0 0 x 0.84 0 y 0.67 0 x 0.83

law is exactly valid within the limits of error Da/a 4 104 and follows the equation (in A) aðxÞ ¼ 6:48220:3792x

ð1:16Þ

CdSxTe1x shows a zinc-blende–wurtzite crystalline phase change at any alloy composition. Early studies failed to grow alloys for the full range of compositions, concluding that a large 6.6

a (Å)

6.5

ZnxCd1-xTe

6.4 6.3 6.2 6.1 6.0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.19 Lattice constant a as a function of x for ZnxCd1xTe at 300 K. The experimental data are taken from Schenk et al. [32]. The solid line represents the linear best fit of Equation (1.16)

STRUCTURAL PROPERTIES

31

miscibility gap exists in the CdS–CdTe pseudobinary system [33]. In 1973 Ohata et al. [34] studied the bulk alloy system for the full range of compositions and reported a change in the crystalline phase at x 0.2. Figure 1.20 plots the lattice constants a and c versus x for bulk CdSxTe1x crystals as measured by Wood et al. [35] using XRD. The composition x of each pellet was determined independently using PIXE. In Figure 1.20, the phase change occurs at x 0.2, in agreement with Ohata et al. [34]. The solid triangles represent the effective cubic lattice parameters aeff ¼ (H3a2c)1/3 defined in Adachi [1]. It can be concluded from Figure 1.20 that the lattice parameters both in the zinc-blende and wurtzite phases obey Vegard law well. It is also understood that if we consider aeff, instead of a or c, in the wurtzite phase (0.2 < x 1.0), CdSxTe1x gives the linear relationship between a and x over the whole alloy range (0 x 1.0). 8 c (w)

a (Å)

7 a (zb) 6 CdSxTe1-x

5

a (w)

4 0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.20 Lattice constants a and c versus x for bulk CdSxTe1x in the zinc-blende (zb) and wurtzite (w) structures at 300 K. The experimental data are taken from Wood et al. [35]. The solid triangles represent the effective cubic parameters aeff ¼ (H3a2c)1/3

Near-neighbor distance (Å)

Motta et al. [36] carried out EXAFS measurements on ZnxCd1xTe. These results are shown in Figure 1.21 by the open circles. The solid circles correspond to the XRD data by Schenk et al. [32]. We can see that the EXAFS bond lengths in Figure 1.21 change much less than the nearest-neighbor distances determined from the XRD. As in the case of the III–Valloys (Figures 1.16 and 1.17), the XRD lattice parameters in II–VI alloys do not reflect the actual bond lengths of the nearest neighbors. The EXAFS data of Motta et al. [36] agreed with a random distribution of atoms in the mixed cation sublattice. 2.85 ZnxCd1-xTe

2.80 2.75

Cd-Te

2.70

Zn-Te

2.65 2.60

0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.21 Near-neighbor distance in ZnxCd1xTe at 300 K. The experimental data (open circles) are taken from Motta et al. [36]. The solid circles represent the bond lengths obtained from the XRD data by Schenk et al. [32]

32

PROPERTIES OF SEMICONDUCTOR ALLOYS

1.5 COHERENT EPITAXY AND STRAIN PROBLEM 1.5.1 Bilayer Model Recent semiconductor devices usually have multilayer structures. The distribution of strains in multilayer structures is the subject of perennial, great interest since internal strains normally arise in thin epitaxial films during the preparation by heteroepitaxial growth. Internal strains or stresses are a consequence of the mismatch of lattice constants and/or the difference in the thermal expansion coefficients of the individual layers. The strain and stress are related through the fourth-rank elastic stiffness [C] or compliance tensor [S] [1]. Let us consider the case of bonding a thin plate of zinc-blende crystal of size Neae Neae te onto a substrate of a different size Nsas Nsas ts, where Ni is the number of lattice atoms along the edge of the crystal plate, ai is the lattice constant and ti is the thickness of the plate; see Figure 1.22(a) [37]. To achieve a coherent interface, Ne is set to equal Ns. Let us assume that ae is less than as and thus le ¼ Neae is less than ls ¼ Nsas. The bonding operation is carried out in the following manner: equal and opposite forces F are applied to the plates to stretch plate ‘e’ and compress plate ‘s’ uniformly in the lateral direction to the same final dimension lf lf. The two plates are then bonded together with a perfect alignment of the atomic planes; see Figure 1.22(b). At the moment when the two plates are bonded together, the composite experiences an applied bending moment given by F(ts þ te)/2, which is counterbalanced by the moment resulting from the internal elastic stress. Finally, the applied forces are relieved, and the moments from the elastic stresses bend the composite in the direction shown in

Figure 1.22 Formation of a two-layer composite: (a) two single-crystalline plates with the lattice constants ae and as (ae < as) and thicknesses te and te, respectively; (b) layer ‘e’ is stretched and layer ‘s’ is compressed to match the macroscopic dimension, and the two layers are then bonded together to form a composite; (c) the composite bends toward the side with the shorter lattice constant after removal of the external stresses Fe and Fs

STRUCTURAL PROPERTIES

33

Figure 1.22(c). The bending of the composite relaxes some of the stress, and the radius of curvature is determined by the final state of the internal stress. Based on this bilayer model, Noyan and Segm€ uller [37] obtained the coherency condition in terms of the curvature radius R 3 ae as 2 ts ae te 1 ae a s Ee t e Es t s Ee ts2 te 1þ þ ¼ 1þ þ R 4 Ee ts te ð1 þ te =ts Þ as as as ts a e Es t s 12 4

ð1:17Þ

where Ei ¼

Yi 1Pi

ð1:18Þ

with Y ¼ Young’s modulus and P ¼ Poisson’s ratio. The term d shown in Figure 1.22(c) represents the shift of the neutral axis of the composite from ts/2. This quantity is given by d¼

te Ee 1 þ te =ts 2Es 1 þ ðEe te =Es ts Þ

ð1:19Þ

Solving the elastic force and momentum balance equations, Noyan and Segm€uller [37] gave the elastic stress component Xxx parallel to the film as e Xxx ¼

Ee as ae as ae te ts 1þ 1 þ ðas Ee te =ae Es ts Þ ae as as ts 2R

ð1:20Þ

The relationship between the film and substrate stresses is given by te e s ¼ Xxx Xxx ts

ð1:21Þ

The dependence of Xxx on z is now given by e e Xxx ðzÞ ¼ Xxx þ Ee

s e Xxx ðzÞ ¼ Xxx

zte =2 R

for

te z þ te =2 þ Es R ts

0 z te

ð1:22aÞ

for

ð1:22bÞ

0 z ts

s e < 0; Xxx > 0, and R < 0. In the case where ae < as, these expressions give Xxx

1.5.2 Elastic Strain and Lattice Deformation Since Xzz is equal to zero in the bilayer model discussed above, the lattices are free to expand or contract in the z direction, that is, perpendicular to the interface. As seen in Figure 1.23, this i i causes the cubic lattice structure to be tetragonally distorted. Since both Xxx and Xyy have opposite signs for i ¼ s compared to i ¼ e, the two cubic lattices are tetragonally distorted in the opposite sense, one with the lattice constant perpendicular to the interface lengthened and

34

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 1.23 Cross section of an ‘epilayer–substrate’ system, where ae and as are the unstrained lattice parameters of the epilayer and substrate, respectively

the other shortened. Therefore, the measured vertical mismatch is enhanced by the tetragonal distortion. Lattice deformation between the epilayer and substrate can be determined by conventional XRD. For example GaxIn1xPyAs1y epilayers on InP(100) are shown in Figure 1.24 [38], where the GaxIn1xPyAs1y/InP samples were grown by LPE with the Ga atomic fractions in liquid solution between 0.4 an 1.0 at%. The experimental lattice deformation Da/a perpendicular to the layer surface for layers with a Ga fraction lower than 0.0065 has a positive value (i.e. compressive strain in the growth direction), while it has negative values (tensile strain) for layers with a fraction larger than 0.0065. In practical cases where the thickness of the epilayer is very small compared to that of the substrate, the lattice mismatch can be taken up totally by the tensile or compressive strain inside the epilayer, giving a coherent interface. A discontinuity in the lattice constant parallel to the interface can exist only in the presence of misfit dislocations. Nagai [39] studied the

Figure 1.24 Lattice mismatch in a GaInPAs/InP heterostructure as a function of the Ga atom fraction in LPE-growth liquid solution. [Reprinted with permission from K. Oe and K. Sugiyama, Appl. Phys. Lett. 33, 449 (1978). Copyright (1978) by the American Institute of Physics]

STRUCTURAL PROPERTIES

35

effects of lattice misfit on the lattice deformation for GaxIn1xAs on GaAs by HT-VPE. The thickness of the substrates was in the range 2–5 mm and the epilayer was in the range 5–10 mm. His results are shown in Figure 1.25, where a|| is the unstrained lattice parameter of the substrate (GaAs) and a? is the strained lattice parameter of the epilayer due to tetragonal distortion.

Figure 1.25 Lattice-constant ratio ae/as for HT-VPE-grown GaxIn1xAs on (1 0 0) and (1 1 1)As planes of GaAs. [Reprinted with permission from H. Nagai, J. Appl. Phys. 45, 3789 (1974). Copyright (1974) by the American Institute of Physics]

The lattice constant of InAs (6.0583 A) is larger than that of GaAs (5.65330 A). Thus, the GaxIn1xAs lattice on GaAs is expected to be tetragonally distorted with the lattice constant perpendicular to the interface being lengthened. The measured lattice constants perpendicular to the film are indeed larger than that along the surface. In the region x > 0.8 the degree of deformation increased with decreasing x, but in the region x < 0.8 it decreased with decreasing x. With the aid of defect revealing etching, it was concluded that in the region x > 0.8 the lattice mismatch is relieved only by tetragonal distortion and for x < 0.8 it is relieved by both misfit dislocation and tetragonal distortion. Figure 1.26 plots the lattice constant a versus x for strained CxSi1x alloy grown on Si(100) by solid-source MBE. The experimental data are taken from Berti et al. [14]. The dash-dotted

a⊥ (Å)

5.44

5.42

CxSi1-x

5.40

5.38 0

0.004 0.008 0.012 0.016 0.020 x

Figure 1.26 Lattice constant a versus x for strained CxSi1x grown on Si(1 0 0) by solid-source MBE. The experimental data are taken from Berti et al. [14]. The dash-dotted line represents the linearly interpolated values between diamond and Si. The light solid and dashed lines are calculated from Equation (1.23) by introducing a0 values estimated from Vegard law between Si and 3C-SiC (x ¼ 0.5) and between Si and C (x ¼ 1.0), respectively. The heavy solid line is calculated by introducing the Monte Carlo-simulated lattice constants reported by Kelires [13] as a0

36

PROPERTIES OF SEMICONDUCTOR ALLOYS

line shows the linear interpolation result between diamond (a ¼ 3.5670 A) and Si (a ¼ 5.4310 A). We can see that the linear interpolation scheme predicts quite different lattice parameters from the experimental data. The strain in the epilayer and hence the lattice constant in growth direction a? can be calculated from the elastic theory [37] 2P a? ¼ ða0 ajj Þ 1 þ ð1:23Þ þ ajj 1P where a0 is the lattice constant of the relaxed material, a|| is the in-plane lattice constant assumed to be the same as the substrate parameter and P is Poisson’s ratio. In the case of cubic materials, Equation (1.23) can be rewritten as 2C12 a? ¼ ða0 ajj Þ 1 þ ð1:24Þ þ ajj C11 where Cij is the elastic stiffness constant. The light solid and dashed lines in Figure 1.26 represent the calculated results of Equation (1.23) by introducing a0 values estimated from Vegard law between Si and 3C-SiC (x ¼ 0.5) and between Si and diamond (x ¼ 1.0), respectively (Figure 1.6). The heavy solid line is also obtained from Equation (1.23) by introducing Monte Carlo-simulated lattice constants [13] as a0. The P values in Equation (1.23) are obtained from the linear interpolation between diamond and Si [1]. The results in Figure 1.26 suggest that the lattice constant a in CxSi1x significantly deviates from Vegard law. The relationship between a and x can be finally given by Equation (1.3). Figure 1.27 shows the lattice parameters perpendicular and parallel to the epilayer surface of MOMBE-grown GaNxAs1x on GaAs(100) [40]. The experimental data clearly suggest that the GaNxAs1x layers are coherently grown on the GaAs(100) substrates. The dashed line is simply estimated from the linear interpolation between c-GaN and GaAs. The solid lines are calculated from Equation (1.23) with a|| ¼ 5.6517 A. The relaxed parameter a0 and Poisson’s ratios used in the calculation are taken from Vegard law between c-GaN and GaAs [1]. We can see in Figure 1.27 excellent agreement between the calculated and experimental lattice parameters.

5.70 a||

a (Å)

5.65 5.60 5.55

a⊥

GaNxAs1-x Vegard law

5.50 0

0.01

0.02

0.03

0.04

0.05

x

Figure 1.27 Lattice parameters perpendicular (a?) and parallel (a||) to the epilayer surface of MOMBEgrown dilute-nitride GaNxAs1x on GaAs(1 0 0). The experimental data are taken from Uesugi et al. [40]. The dashed line is simply estimated from Vegard law between c-GaN and GaAs. The solid lines are calculated from Equation (1.23) with a|| ¼ 5.6517 A (const.). The relaxed parameters a0 and Poisson’s ratios P are taken from Vegard law between c-GaN and GaAs

STRUCTURAL PROPERTIES

37

The essentially same analysis as in Figure 1.27 is performed on strained AlxGa0.9xIn0.1N grown by MOCVD [24]. The solid line in Figure 1.14 represents the result of this analysis. Note that Poisson’s ratio is a crystallographic plane- and direction-dependent quantity. The expressions of Poisson’s ratio P and corresponding numeric values for some hexagonal semiconductors are summarized in Tables 3.19 and 3.20 of Adachi [1]. The quaternary P values used in Equation (1.23) are estimated from Vegard law. The in-plane lattice constant a|| is assumed to be 5.240 A. In Figure 1.14, there is good agreement between the calculated and experimental values even in the wurtzite crystal structure. However, in the case of relaxed AlxIn1xN alloy Vegrad law leads to an overestimation of the In mole fraction, which cannot be explained by either strain state or impurity levels. The In atomic fraction can be overestimated by as much as 6–37% in the range of 0.18 < x < 0.93 [41]. Figures 1.28(a) and 1.28(b) show the experimental lattice parameters a and c for MgxZn1xO layers on sapphire (0001) [42] and on 6H-SiC (0001) [43]. The solid lines show the linear interpolation results of c and a between MgO and ZnO. The effective cubic lattice parameters aeff ¼ (H3a2c)1/3 for MgO and ZnO are, respectively, 4.484 and 4.567 A, while those for sapphire and 6H-SiC are 6.335 A and 4.359 A, respectively. Coherently grown MgxZn1xO films on the sapphire and 6H-SiC substrates will be tensile- and compressive-strained, respectively. The ZnO (x ¼ 0) layers, however, exhibited virtually relaxed lattice constants of 3.246 and 5.205 A along the a and c axes, respectively. As seen in Figure 1.28, the c- (a-) axis length decreased (increased) with increasing x for MgxZn1xO both on the sapphire and 6H-SiC substrates. The resulting ratio c/a decreased with increasing x, indicating that the MgxZn1xO films are considerably distorted from the ideal wurtzite although they are in the relaxed states.

Figure 1.28 (a) a-axis and (b) c-axis lattice parameters at 300 K for MgxZn1xO grown on Al2O3 (0001) substrate by Ohtomo et al. [42] and on 6H-SiC (0001) substrate by Ashrafi and Segawa [43]. The solid lines in (a) and (b) show the linearly interpolated values of a and c between MgO and ZnO. The corresponding c/a ratios are plotted in (c)

1.5.3 Critical Thickness Pseudomorphic epitaxy, in which a high-quality thin film is epitaxially grown on a latticemismatched substrate, has found its application in many areas [44]. SLs and QWs are high-quality multilayered structures grown from lattice matched and mismatched materials.

38

PROPERTIES OF SEMICONDUCTOR ALLOYS

The large lattice mismatch is totally accommodated by uniform elastic strains in the layers if the layer thicknesses are kept below certain critical values. The idea for thin films emerged from a critical layer thickness hc below which a dislocation-free, coherently strained interface would be stable and above which a misfit dislocation structure and semi-coherent interface would be stable. Knowledge of the so-called critical thickness is essential for realizing the advantages of lattice-mismatched heterostructure systems. The critical thickness hc of an epilayer, which was first considered by Frank and van der Merwe [45], is a parameter introduced to explain the experimental observation of coherent, pseudomorphic or strained-layer epitaxy. The breakdown of coherency can be determined in several ways. XRD and PL are commonly employed methods of determining the loss of coherency by demonstrating a change in average lattice constant (XRD) or a shift in PL peak energy and a reduction in PL intensity, following the release of strain. TEM is the direct manifestation of the breakdown of coherency. We show in Figure 1.29 the critical thickness hc versus x for (a) SixGe1x layer on Si, (b) GaxIn1xAs layer on InP and (c) GaNxAs1x layer on GaAs, respectively. Note that x ¼ 0.47 in Figure 1.29(b) is the lattice-matching composition to InP. 104

(a) SixGe1-x /Si

102

hc (Å)

100

0

104

0.2

0.4

0.6

0.8

1.0

0.6

0.8

1.0

(b) Gax In1-x As/InP

102 100

0

0.2

0.4

104

(c) GaNx As1-x /GaAs

102 100

0

0.02

0.04

0.06

0.08

0.10

x

Figure 1.29 Critical thickness hc versus x for (a) SixGe1x layer on Si, (b) GaxIn1xAs layer on InP and (c) GaNxAs1x layer on GaAs. The solid lines represent the theoretical model of Matthews and Blakeslee [46]. The heavy solid line in (a) is obtained from an energy-balanced misfit dislocation generation model by People and Bean [47]

Although several theories have been proposed to predict hc [44], most semiconductor device designers rely upon the model of Matthews and Blakeslee [46]. The solid lines in Figure 1.29 show the results based on this model. The experimental hc data usually exceed the Matthews–Blakeslee’s prediction. It is also understood that for SixGe1x there is little dependence of hc on x. The heavy solid line in Figure 1.29(a) represents the theoretical curve obtained from an energy-balanced misfit dislocation generation model by People and Bean [47]. This model is in excellent agreement with the experimental data. The critical thicknesses hc for AlxGa1xN and GaxIn1xN on relaxed GaN layers were measured by Akasaki and Amano [48]. The experimental hc values were in the range 300 to 700 nm for AlxGa1xN/GaN (0.05 x 0.2) and 40 nm for GaxIn1xN/GaN (0.8 x 0.95).

STRUCTURAL PROPERTIES

39

The hc values for SixGe1x/Si and some III–V and II–VI semiconductors grown on various lattice-mismatched substrates are summarized in Figure 1.30. The solid lines are obtained by least-squares fitting with (hc in A, Da/a in at%) A n hc ¼ ð1:25Þ Da=a with A ¼ 7.5 and n ¼ 3.5 for SixGe1x/Si, A ¼ 16 and n ¼ 2.4 for III–V semiconductors and A ¼ 52 and n ¼ 1.5 for II–VI semiconductors. It should be noted that the II–VI semiconductors have weak bond strength. The dislocation energy in such semiconductors is much smaller than those in SixGe1x/Si and III–V semiconductors. Therefore, dislocations can be more easily generated in the II–VI semiconductors. 104

(a) SixGe1-x /Si

102

hc (Å)

100 104 102

(b) III-V semiconductors

100 104 102

(c) II-VI semiconductors 100 -2 10 10-1 100 Δa/a (%)

101

Figure 1.30 Critical thickness hc for (a) SixGe1x, (b) III–V and (c) II–VI semiconductors grown on various lattice-mismatched substrates. The solid lines represent the least-squares fit using Equation (1.25)

1.6 STRUCTURAL PHASE TRANSITION At high pressure the group-IV elemental semiconductors show metallic transitions in a sequence from cubic (diamond) ! tetragonal (b-Sn) ! simple hexagonal ! hexagonal close packed. Similarly, the III–V and II–VI binary semiconductors exhibit a variety of the crystal structures at high pressures. In Tables 1.8 and 1.9 of Adachi [1], transition pressure to the first phase (PT) and transition sequences can be found for some group-IV, III–V and II–VI semiconductors. The additional data are: PT ¼ 56 GPa (zinc-blende ! hexagonal (NiAs)) for BeSe; PT ¼ 35 GPa (zincblende ! hexagonal (NiAs)) for BeTe; and PT ¼ 90.6 GPa (rocksalt ! CsCl) for CdO. There are a very few studies on the structural phase transition in semiconductor alloys. Some of these studies are summarized in Table 1.16. Webb et al. [49] observed the phase transition in ZnxCd1xTe from the zinc-blende to rocksalt structures. However, the recent studies on ZnTe and CdTe suggest the presence of cinnabar phase between the zinc-blende and rocksalt structures [50]. Vnuk et al. [51] studied the effect of pressure on semiconductor

40

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.16 Phase-transition sequence observed for some III–V and II–VI ternaries at high pressures. zb ¼ zinc-blende; or ¼ orthorhombic; w ¼ wurtzite; rs ¼ rocksalt (NaCl); cin ¼ cinnabar System

Material

Sequence

Ref.

III–V

GaxIn1xP AlxGa1xAs GaxIn1xSb

semiconductor ! metal (optical absorption) zb ! or (Pmm2)/or (Cmcm) (GaAs like) zb ! b-Sn

a b c

II–VI

MgxZn1xO ZnxCd1xS ZnxCd1xSe

w ! rs zb ! rs zb ! rs (x ¼ 0.9) semiconductor ! metal (0 x 0.32) zb ! rs semiconductor ! metal (resistance) zb ! cin ! rs (0 x 0.55) zb ! rs (0.55<x 1)

d e f g h i j j

ZnxCd1xTe ZnSxSe1x ZnSexTe1x

A. R. Go~ ni et al., Phys. Rev. B 39, 3178 (1989) W. Paszkowicz et al., Acta Phys. Pol. A, 91, 993 (1997) c C. Y. Liu et al., J. Phys. Chem. Solids 39, 113 (1978) d J. A. Sans and A. Segura, High Pressure Res. 24, 119 (2004) e A. Beliveau and C. Carlone, Phys. Rev. B 44, 3650 (1991) f C.-M. Lin et al., Phys. Rev. B 58, 16 (1998) g Y. C. Lin et al., J. Appl. Phys. 101, 073507 (2007) h A. W. Webb et al., J. Appl. Phys. 61, 2492 (1987) i S. R. Tiong et al., Jpn. J. Appl. Phys. 28, 291 (1989) j J. Pellicer-Porres et al., Phys. Rev. B 71, 035210 (2005) a b

(a-Sn)-to-metal (b-Sn) transition temperature in dilute GexSn1x (x 1 at%). They obtained a slope of 48.4 6 K/kbar, in good agreement with thermodynamic prediction. Figure 1.31 plots the transition pressure to the first phase PT versus x for GaxIn1xSb. The experimental data are taken from Liu et al. [52]. A slight bowing can be found in the PT versus

7

PT (GPa)

6 5

β -Sn

4 3

zb

2 Gax In1-x Sb

1 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.31 Transition pressure to the first phase PT versus x for GaxIn1xSb. The experimental data are taken from Liu et al. [52]. The solid line shows the quadratic-fit result using Equation (1.26). zb ¼ zinc-blende

STRUCTURAL PROPERTIES

41

x plots. The solid line shows the best-fit result of the quadratic expression (in GPa) PT ðxÞ ¼ 2:3 þ 6:5x2:6x2

ð1:26Þ

PT (GPa)

The transition pressures to the first phase PT against alloy composition x for some II–VI semiconductors are shown in Figure 1.32. The experimental data are taken for ZnxCd1xS from Beliveau and Carlone [53], for ZnSxSe1x from Tiong et al. [54] and for ZnSexTe1x from Pellicer-Porres et al. [55]. In Figure 1.32(c), the transition pressure to the second phase is also plotted with the open circles. The linear interpolation is concluded to be an efficient tool to estimate the phase transition pressure in semiconductor alloys. 20 15 10 5 0 16 15 14 13 12 20

(a) ZnxCd1-xS

zb m

(b) ZnSxSe1-x

s

rs

cin

15 10 5

rs

zb

0

0.2

0.4

(c) ZnSexTe1-x x

0.6

0.8

1.0

Figure 1.32 Transition pressures to the first phase PT against x for (a) ZnxCd1xS, (b) ZnSxSe1x and (c) ZnSexTe1x. The transition pressure to the second phase is plotted in (c) by the open circles. The experimental data are taken for (a) ZnxCd1xS from Beliveau and Carlone [53], for (b) ZnSxSe1x from Tiong et al. [54] and for (c) ZnSexTe1x from Pellicer-Porres et al. [55]. cin ¼ cinnabar; m ¼ metal; rs ¼ rocksalt (NaCl); s ¼ semiconductor; zb ¼ zinc-blende

1.7 CLEAVAGE PLANE 1.7.1 Cleavage The cleavage properties of a crystal are strongly related to the atomic arrangement and corresponding electron density map. The most readily cleaved crystallographic planes can then be determined only by the crystalline structure. They are (111) plane for alloys of diamond type, (1 1 0) plane for zinc-blende type, ð11 20Þ and ð1010Þ planes for wurtzite type and (100) plane for rocksalt type [1].

1.7.2 Surface Energy The cleavage energy is assumed equal to twice the surface energy of that plane. There is a dearth of experimental measurements on surface energy. The surface energies for several group-VI elemental, III–Vand II–VI binary semiconductors are listed in Tables 1.11–1.13 of Adachi [1]. No surface energy data are available for semiconductor alloys.

42

PROPERTIES OF SEMICONDUCTOR ALLOYS

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons Ltd, Chichester, 2005. [2] A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys, Kluwer Academic, New York, 2002. [3] A. Ourmazd and J. C. Bean, Phys. Rev. Lett. 55, 765 (1985). [4] J. Schilz and V. N. Romanenko, J. Mater. Sci.: Mater. Electron. 6, 265 (1995). [5] T. S. Kuan, T. F. Kuech, W. I. Wang, and E. L. Wilkie, Phys. Rev. Lett. 54, 201 (1985). [6] T. Suzuki, in A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys, Kluwer Academic, New York, 2002, p. 1. [7] A. Gomyo, M. Sumino, I. Hino, and T. Suzuki, Jpn. J. Appl. Phys. 34, L469 (1995). [8] A. Gomyo, K. Makita, I. Hino, and T. Suzuki, Phys. Rev. Lett. 72, 673 (1994). [9] A. A. Mbaye, L. G. Ferreira, and A. Zunger, Phys. Rev. Lett. 58, 49 (1987). [10] H. S. Lee, S. Yi, T. W. Kim, Y. J. Park, J. Y. Lee, M. S. Kwon, and H. L. Park, Solid State Commun. 137, 70 (2006). [11] R. A. Soref, Proc. IEEE 81, 1687 (1993). [12] E. T. Croke, A. T. Hunter, C. C. Ahn, T. Laursen, D. Chandrasekhar, A. E. Bair, D. J. Smith, and J. W. Mayer, J. Cryst. Growth 175–176, 486 (1997). [13] P. C. Kelires, Phys. Rev. B 55, 8784 (1997). [14] M. Berti, D. D. Salvador, A. V. Drigo, F. Romanato, J. Stangl, S. Zerlauth, F. Sch€affler, and G. Bauer, Appl. Phys. Lett. 72, 1602 (1998). [15] J. P. Dismukes, L. Ekstrom, and R. J. Paff, J. Phys. Chem. 68, 3021 (1964). [16] M. Matsuura, J. M. Tonnerre, and G. S. Cargill III, Phys. Rev. B 44, 3842 (1991). [17] H. Kajiyama, S. Muramatsu, T. Shimada, and Y. Nishino, Phys. Rev. B 45, 14005 (1992). [18] I. Yonenaga, M. Sakurai, M. H. F. Sluiter, Y. Kawazoe, and S. Muto, J. Mater. Sci.: Mater. Electron. 16, 429 (2005). [19] N. S. Takahashi, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 3. [20] R. E. Nahory, M. A. Pollack, W. D. Johnston, Jr., and R. L. Barns, Appl. Phys. Lett. 33, 659 (1978). [21] F. Germini, C. Bocchi, C. Ferrari, S. Franchi, A. Baraldi, R. Magnanini, D. D. Salvador, M. Berti, and A. V. Drigo, J. Phys. D: Appl. Phys. 32, A12 (1999). [22] J. D. Bearch, H. Al-Thani, S. McCray, R. T. Collins, and J. A. Turner, J. Appl. Phys. 91, 5190 (2002). [23] L. T. Romano, B. S. Krusor, M. D. McCluskey, and D. P. Bour, Appl. Phys. Lett. 73, 1757 (1998). [24] M. E. Aumer, S. F. LeBoeuf, F. G. McIntosh, and S. M. Bedair, Appl. Phys. Lett. 75, 3315 (1999). [25] G. Bisognin, D. D. Salvador, C. Mattevi, M. Berti, A. V. Drigo, G. Ciatto, L. Grenouillet, P. Duvaut, G. Gilet, and H. Mariette, J. Appl. Phys. 95, 48 (2004). [26] S. Z. Wang, S. F. Yoon, W. J. Fan, W. K. Loke, T. K. Ng, and S. Z. Wang, J. Appl. Phys. 96, 2010 (2004). [27] G. Fournet, J. Phys. Radium 14, 374 (1953). [28] J. C. Mikkelsen, Jr., and J. B. Boyce, Phys. Rev. Lett. 49, 1412 (1982); Phys. Rev. B 28, 7130 (1983) [29] H. Oyanagi, Y. Takeda, T. Matsushita, T. Ishiguro, and A. Sasaki, in Gallium Arsenide and Related Compounds, IOP, Bristol, 1986, p. 295. [30] N. J. Jeffe, A. V. Blant, T. S. Cheng, C. T. Foxon, C. Bailey, P. G. Harrison, J. F. W. Mosselmans, and A. J. Dent, Mater. Res. Soc. Symp. Proc. 512, 519 (1998). [31] T. Mattila and A. Zunger, J. Appl. Phys. 85, 160 (1999). [32] M. Schenk, I. H€ahnert, L. T. H. Duong, and H.-H. Niebsch, Cryst. Res. Technol. 31, 665 (1996). [33] E. Cruceanu and D. Niculesciu, Compt. Rend. Acad. Sci. 261, 935 (1965). [34] K. Ohata, J. Saraale, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1198 (1973). [35] D. A. Wood, K. D. Rogers, D. W. Lane, G. J. Conibeer, and D. Parton, J. Mater. Sci. Lett. 17, 1511 (1998).

STRUCTURAL PROPERTIES

43

[36] N. Motta, A. Balzarotti, P. Letardi, A. Kisiel, M. T. Czyzyk, M. Zimnal-Starnawska, and M. Podgorny, Solid State Commun. 53, 509 (1985). [37] I. C. Noyan and A. Segm€uller, J. Appl. Phys. 60, 2980 (1986). [38] K. Oe and K. Sugiyama, Appl. Phys. Lett. 33, 449 (1978). [39] H. Nagai, J. Appl. Phys. 45, 3789 (1974). [40] K. Uesugi, N. Morooka, and I. Suemune, Appl. Phys. Lett. 74, 1254 (1999). [41] T. Sepp€anen, L. Hulman, J. Birch, M. Beckers, and U. Kreissig, J. Appl. Phys. 101, 043519 (2007). [42] A. Ohtomo, M. Kawasaki, T. Koida, K. Masubuchi, H. Koinuma, Y. Sakurai, Y. Yoshida, T. Yasuda, and Y. Segawa, Appl. Phys. Lett. 72, 2466 (1998). [43] A. B. M. A. Ashrafi and Y. Segawa, J. Vac. Sci. Technol. B 23, 2030 (2005). [44] S. Jain, M. Willander, and R. Van Overstraeten, Compound Semiconductors Straiend Layers and Devices. Kluwer Academic. Boston, 2000. [45] F. C. Frank and J. H. van der Merwe, Proc. Roy. Soc. A 201, 261 (1950). [46] J. W. Matthews and A. E. Blakeslee, J. Cryst. Growth 27, 118 (1974). [47] R. People and J. C. Bean, Appl. Phys. Lett. 49, 229 (1986). [48] I. Akasaki and H. Amano, in Semiconductors and Semimetals, Vol. 50 (edited by J. I. Pankove and T. D. Moustakas), Academic, New York, 1998, p. 459. [49] A. W. Webb, S. B. Qadri, E. R. Carpenter, Jr., E. F. Skelton, and J. Kennedy, J. Appl. Phys. 61, 2492 (1987). [50] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Semiconductors. Kluwer Academic, Boston, 2004. [51] F. Vnuk, A. D. Monte, and R. W. Smith, J. Appl. Phys. 55, 4171 (1984). [52] C. Y. Liu, I. L. Spain, and E. F. Skelton, J. Phys. Chem. Solids 39, 113 (1978). [53] A. Beliveau and C. Carlone, Phys. Rev. B 44, 3650 (1991). [54] S. R. Tiong, M. Hiramatsu, Y. Matsushima, and E. Ito, Jpn. J. Appl. Phys. 28, 291 (1989). [55] J. Pellicer-Porres, D. Martınez-Garcıa, Ch. Ferrer-Roca, A. Segura, and V. Mu~ noz-Sanjose, Phys. Rev. B 71, 035210 (2005).

2 Thermal Properties 2.1 MELTING POINT AND RELATED PARAMETERS 2.1.1 Phase Diagram (a) Group-IV semiconductor alloy Figure 2.1 shows the phase diagram for the Si–Ge system at temperatures near the melting point. The experimental data are taken from various sources. The solid lines show the quadratic fit results (in C) Solidus surface :

Ts ðxÞ ¼ 937 þ 244x þ 231x2

ð2:1aÞ

Liquidus surface :

Tl ðxÞ ¼ 937 þ 916x442x2

ð2:1bÞ

The phase diagram in Figure 2.1 suggests that Si and Ge are completely miscible as liquid and as solid. Stable phases formed by Si and Ge are the liquid and a cubic diamond-type substitutional solid solution. No phase changes or decompositions were detected roentgenographically after annealing homogeneous SixGe1x solid solutions for several months at temperatures in the range 177–925 C [1]. At high pressures above 15 GPa, the bct structure of a Si–Ge solid solution is estimated to be more stable than the diamond structure [2]. The Si–Ge system is a typical representative of a system with strong segregation, i.e. a solid solution in which the solid and liquid phases are separated by a large regime of coexistence. (b) III–V semiconductor alloy A series of papers demonstrated the feasibility of calculating phase diagrams in III–V ternary systems based upon the regular or quasichemical equilibrium model for the solid and liquid phases [3–5]. Because of the small lattice difference between GaAs and AlAs, their solid solutions are the closest in the III–V semiconductor systems to being ideal and the alloys are among the easiest to prepare by LPE. A perspective diagram depicting the solidus surface, liquidus surface and binary boundaries of the Al–Ga–As ternary system is shown in Figure 2.2(a). Figure 2.2(b) also shows the pseudobinary phase diagram of AlAs–GaAs system. We can see in Figure 2.2 that AlAs and GaAs are completely miscible as liquid and as solid. Stable phases formed by these binary compounds are the liquid and a cubic zinc-blende substitutional solid solution of Al and Ga atoms in the cation site. The solid lines in Figure 2.2(b) represent the solidus and liquidus surfaces (in C) [6] Solidus surface : Liquidus surface :

Ts ðxÞ ¼ 123854x þ 560x2

ð2:2aÞ

Tl ðxÞ ¼ 1238 þ 1082x580x2

ð2:2bÞ

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

46

PROPERTIES OF SEMICONDUCTOR ALLOYS 1500 1400

SixGe1-x

1300 T (°C)

Liquid 1200 1100

Solid + Liquid

1000 Solid

900 800

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.1 Normal-pressure phase diagram of a Si–Ge system. The solid lines represent the quadratic fits using Equation (2.1)

Figure 2.2 (a) Perspective diagram depicting the solidus surface, liquidus surface and binary boundaries in the Al–Ga–As ternary system. (b) Solidus and liquidus curves for the AlAs–GaAs pseudobinary system. The solid lines in (b) represent the solidus and liquidus surfaces calculated from Equation (2.2)

Figure 2.3 shows the solidus and liquidus curves for (a) GaP–InP, (b) GaAs–InAs and (c) GaSb–InSb systems. These systems provided a homogeneous series of alloys differing only in the anion substitution. The pseudobinary GaSb–InSb system can be approximated by the quadratic expressions (in C) Solidus surface :

Ts ðxÞ ¼ 52472x þ 261x2

ð2:3aÞ

Liquidus surface :

Tl ðxÞ ¼ 524 þ 280x90x2

ð2:3bÞ

This is not the case for the GaP–InP and GaAs–InAs systems, as seen in Figures 2.3(a) and 2.3(b).

THERMAL PROPERTIES

47

1600 (b) GaxIn1-xAs

Liquid

(c) GaxIn1-xSb

1400 Liquid

T (°C)

1200 1000 Solid

Solid

800

Liquid

600 (a) GaxIn1-xP

Solid

400 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x

Figure 2.3 Solidus and liquidus curves for (a) GaP–InP, (b) GaAs–InAs and (c) GaSb–InSb pseudobinary systems. The solid lines in (c) represent the solidus and liquidus surfaces calculated from Equation (2.3)

GaxIn1xN is a random alloy having the wurtzite structure. Due to the large difference (11%) in the lattice constants between GaN and InN, the solid solution has a tendency to undergo phase separation. It is possible to grow thin epitaxial GaxIn1xN layers with the cubic structure. The phase stability of GaxIn1xN has been the subject of several experimental [7,8] and theoretical studies [9–15]. We reproduce in Figure 2.4 the pseudobinary diagram of zinc-blende and wurtzite GaxIn1xN obtained theoretically by Gan et al. [15]. A direct comparison of the predicted phase diagram to an experimental phase diagram cannot be made since the latter has never been determined. However, an experimental study on Ga0.91In0.09N [8] suggested that this alloy does 1800 Zinc-blende

T (K)

1600

1400

Wurtzite

1200

GaxIn1-xN

1000 0

0.2

0.4

x

0.6

0.8

1.0

Figure 2.4 Pseudobinary phase diagram of zinc-blende and wurtzite GaxIn1xN. The solid and open circles represent the experimental data for which phase separation was and was not observed, respectively; data taken from Doppalapudi et al. [8]. [Reprinted with kind permission from C. K. Gan, Y. P. Feng, and D. J. Srolovitz, Phys. Rev. B 73, 235214 (2006). Copyright (2006) by the American Physical Society]

48

PROPERTIES OF SEMICONDUCTOR ALLOYS

not phase separate at the growth temperature of 923 K. The corresponding data point (x, T) ¼ (0.09, 923 K) is shown by the open circle in Figure 2.4. It lies in the region between the binodal and spinodal, suggesting that the solid solution is metastable with respect to phase segregation. Additional experimental points in Figure 2.4 show that phase separation occurs in both Ga0.63In0.37N and Ga0.65In0.35N grown at 998 K (solid circles) [8], in agreement with the predicted phase diagram (i.e. the data fall in the spinodal region). Gan et al. [15] suggested that the wurtzite structure is thermodynamically more stable than the zinc-blende structure at all temperatures and alloy compositions. They also demonstrated that the lattice vibrations can drastically alter the thermodynamic properties and phase diagram of GaxIn1xN. (c) II–VI semiconductor alloy Figure 2.5 shows the phase diagram of the MgO–ZnO system at 4.4 GPa (solid lines) and at ambient pressure (dashed lines). The ambient and high-pressure diagrams are taken from Raghavan et al. [16] and Solozhenko et al. [17], respectively. At ambient pressure [16], the MgO–ZnO system is of eutectic type and is characterized by the extensive solubility of ZnO in MgO and the restricted solubility of MgO in ZnO. The two-phase region in the MgO–ZnO system extends from 3.5 to 70.5 mol% ZnO at 1000 C and becomes narrower at higher temperatures. Solozhenko et al. [17] observed a phase transition of w-MgxZn1xO solid solution into rocksalt by stepwise heating at various temperatures. The quenching of the 4000 Mgx Zn1-xO L 3400 L+rs-MZO

T (ºC)

2800

2200 rs-MZO

rs-MZO + w-MZO

1600

w-MZO 1000 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.5 Phase diagram of MgO–ZnO pseudobinary system at ambient pressure taken from Raghavan et al. [16] (dashed lines) and at 4.4 GPa (solid lines). MZO ¼ MgZnO; L ¼ liquid; rs ¼ rocksalt; w ¼ wurtzite. [Reprinted with permission from V. L. Solozhenko et al., Solid State Commun. 138, 534–537 (2006), Copyright (2006) Elsevier]

THERMAL PROPERTIES

49

reaction mixtures resulted in the formation of stable MgxZn1xO solid solutions with the rocksalt structure. The phase diagram at 4.4 GPa in Figure 2.5 was proposed based on these facts [17]. Figure 2.6 shows the ZnTe–CdTe solidus and liquidus curves. The experimental data are taken from Steininger et al. [18]. XRD measurements indicated that ZnxCd1xTe forms a complete series of solid solutions with lattice parameters varying almost linearly with x. The solidus and liquidus curves in Figure 2.6 represent monotonic and sublinear variations with x from the melting point of CdTe to that of ZnTe. This type of x versus T variation suggests small and nearly comparable positive deviations from ideality in the solid and liquid phases and is similar to those observed in other II–VI systems, such as ZnSe–ZnTe [19], CdSe–CdTe [20] and HgSe–HgTe (Figure 2.9).

T (°C)

1300

ZnxCd1-xTe

Liquid

1200

Solid 1100 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.6 Solidus and liquidus curves for ZnTe–CdTe pseudobinary system. The experimental data are taken from Steininger et al. [18]. The solid lines represent the solidus and liquidus surfaces calculated from Equation (2.4)

The solid lines in Figure 2.6 represent the quadratic expressions (in C) Solidus surface : Ts ðxÞ ¼ 1092 þ 30x þ 173x2 Liquidus surface : Tl ðxÞ ¼ 1092 þ 131x þ 72x2

ð2:4aÞ ð2:4bÞ

Of particular interest in Figure 2.6 is the slow increase in liquid temperatures and the relatively narrow gap between solidus and liquidus curves (less than 0.16 mole fraction). These are very favorable for the growth of alloys from the melts in standard quartz ampoules up to relatively high values of Zn content [21]. The CdS–CdTe system has different crystal structures, that is, the zinc-blende and wurtzite structures, when prepared high temperatures. Early studies on this alloy system failed to produce mixed crystals for the full range of compositions, concluding that a large miscibility gap exists in the CdS–CdTe system. More recently, Ohata et al. [22] studied the system for the full range of compositions and observed a change of phase from the zinc-blende to wurtzite at x 0.2. Wood et al. [23] confirmed using PIXE and XRD that bulk CdSxTe1x alloy has the zinc-blende structure for x 0.2 and the wurtzite structure for x 0.25. Figure 2.7 shows the phase diagram of the CdS–CdTe system obtained by these authors [22,23]. Figure 2.8 illustrates the phase diagram for the CdSe–CdTe system [21]. This system and the ZnTe–CdTe system in Figure 2.6 show typical ‘lens-shape’ phase diagrams with sublinear

50

PROPERTIES OF SEMICONDUCTOR ALLOYS

CdSxTe1-x

1400

Liquid

Liquid+ Solid

T (ºC)

1200

1000 Wurtzite 800

Zinc-blende+ Wurtzite

Zinc-blende 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.7 Phase diagram of CdS–CdTe pseudobinary system. The experimental curves are taken from Ohata et al. [22] and Wood et al. [23]

variations in temperature with composition and relatively narrow solidus–liquidus gaps. The CdSe–CdTe system represents almost the same type of solidus–liquidus diagram with a degenerate eutectic near 20 mol% CdSe. The narrow zincblende–wurtzite two-phase region inside the solidus field shows increasing stability of the wurtzite phase with increasing temperature.

Figure 2.8 Phase diagram of CdSe–CdTe pseudobinary system. [Reprinted with permission from J. Cryst. Growth, Phase diagrams and crystal growth of pseudobinary alloy semiconductors by J. Steininger and A. J. Strauss, 13–14, 657. Copyright (1972), Elsevier]

THERMAL PROPERTIES

51

800 HgSexTe1-x 750 T (°C)

Liquid

700

Solid

650 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.9 Phase diagram of HgSe–HgTe pseudobinary system. The experimental data are taken from Harman [24]. The solid lines represent the solidus and liquidus surfaces calculated from Equation (2.5)

Harman and Strauss [24] determined the phase diagram for the HgSe–HgTe system. The liquidus data in Figure 2.9 were measured by differential thermal analysis of cooling curves, while the solidus points were obtained by determining the composition of the alloys that were the first to freeze from melts of known composition [24]. The solidus and liquidus curves show a very small separation (about 3 mol% between 25 and 75 mol% HgSe). The solid lines in Figure 2.9 represent the quadratic expressions (in C) Solidus surface : Liquidus surface :

Ts ðxÞ ¼ 67012x þ 141x2

ð2:5aÞ

2

ð2:5bÞ

Tl ðxÞ ¼ 670 þ 3x þ 127x

2.1.2 Melting Point The melting point Tm is one of the most essential thermophysical parameters. Some thermophysical parameters, including Tm, for a number of group-IV, III–Vand II–VI semiconductors are summarized in Table 2.1. Figure 2.10 shows the melting point Tm versus x for CxSi1x. The open circles show the experimental data for diamond and Si, while the solid circle represents the 3C-SiC (x ¼ 0.5) data. The solid line represents Vegard law. It predicts generally acceptable alloy values. We have, however, already shown in Section 2.1.1 that a quadratic function or a higher-order polynomial can be fitted to the solidus curves of many alloys. Therefore, attention should be paid to the estimation of Tm using the linear interpolation scheme.

2.2 SPECIFIC HEAT 2.2.1 Group-IV Semiconductor Alloy Specific heat is a strongly temperature-dependent quantity [25]. There has been no experimental data on the specific heat of group-IV semiconductor alloys. Kagaya et al. [26]

52

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 2.1 Melting point Tm, specific heat Cp, Debye temperature uD, thermal expansion coefficient ath and thermal conductivity K for some group-IV, III–V and II–VI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)); rs ¼ rocksalt; rh ¼ rhombohedral System

Material

Tm (K)

Cp (J/g K)

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb) 2H-SiC (w)

4100a 1687 1210.4

0.5148 0.713 0.3295b 0.278c 0.677e

1870 643 348b 238c 1122

III–V

II–VI

2810 2810

uD (K)

BN (zb) BN (h)

> 3246 > 3246

0.643 0.805

1613 323

BP (zb) BAs (zb) AlN (zb) AlN (w)

> 3300 2300 3487 3487

0.75 0.408

1025i 800

0.728

988

AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaN (w)

2823 2013 1338 2791 2791

0.727 0.424 0.326b

687 450 370b

0.42

821

GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InN (w)

1730 1513 991 2146 2146

0.313 0.327 0.344b

493k 370 240b

2.274

674

InP (zb) InAs (zb) InSb (zb)

1335 1210 797

0.322 0.352 0.350b

420b 280b 161b

BeO (w)

2851

1.029

1280

0.83

900

3250 2783o 1560 > 1300 1975 1975

0.928

745

0.497

416

2196

0.486

440

BeS (zb) BeTe (zb) MgO (rs) MgS (rs) MgSe (zb) MgTe (w) ZnO (zb) ZnO (w) ZnS (zb)

ath (106 K1) 1.05 2.616 5.75 5.25d 2.77 1.15 2.75 (?c) 38.0 (jjc) 2.94 3.042 (?c) 2.227 (jjc) 4.28 4.2j 5.0 (?c) 4.5 (jjc) 4.89 6.03 6.35 3.830 (?c) 2.751 (jjc) 4.56 5.50m 5.04 7.2 (?c)n 6.0 (jjc)n 7.66 10.5

4.31 (?c) 2.49 (jjc) 6.71

K (W/cm K) 22 1.56 0.6 3.4f 13g 3.9h 3.5 3.19h 0.9 0.91 0.57 1.95h 0.77 0.45 0.36 0.45h,l 0.68 0.3 0.165–0.185 3.7h

0.52

0.54h 0.27 (continued)

THERMAL PROPERTIES

53

Table 2.1 (Continued ) System

Material

Tm (K)

ZnS (w)

2196

ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdS (w)

1793 1568 1700 1748 1748

CdSe (zb) CdSe (w)

1531 1531

CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

1365 1723 1072 943

Cp (J/g K)

uD (K) 351

ath (106 K1)

K (W/cm K)

6.54 (?c) 4.59 (jjc) 7.8 8.33 14

0.17h,p

0.20h,q

0.360 0.258 0.340

340 260 255

0.3280

310

4.30 (?c) 2.77 (jjc)

0.281

135

0.211

185

0.355 0.162

242 143

4.13 (?c) 2.76 (jjc) 4.70 4.3r 1.41 4.70

0.19 0.18 0.007

0.09h 0.075 0.001–0.035 0.0238

At 12.5 GPa At 273 K c At 100 K d At 220 K e Cv value f At 290 K g Estimated h This semiconductor has two tensor components, K? and Kjj; however, the difference between K? and Kjj appears to be less than the experimental uncertainty at room temperature i At 320 K j At 280 K k At 150 K l Ceramics m Obtained from an analysis of GaInPAs quaternary data n At 373 K o Theoretical p Note that the w-ZnS crystal used in the experiment may be faulted; therefore, the value for this crystal is much smaller than that for c-ZnS q At 283 K r T ¼ 484 621 K a b

investigated theoretically the specific heat of SixGe1x from 0 to 500 K. The difference in specific heat between at constant pressure and constant volume Cp–Cv was found to be negligible at low temperatures, but increased by less than 3–3.5% at 500 K. The calculated Cp values fell between the endpoint values of Si and Ge. Figure 2.11 shows the specific heat Cp versus x for CxSi1x at 300 K. The experimental data for diamond, Si and 3C-SiC (x ¼ 0.5) are shown by the open and solid circles. The dashed line represents the linear interpolation result between the experimental diamond and Si values written as (in J/g K) Cp ðxÞ ¼ 0:7130:198x

ð2:6Þ

54

PROPERTIES OF SEMICONDUCTOR ALLOYS 5000 4000

CxSi1-x

Tm (K)

3000 2000 3C-SiC 1000 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.10 Melting point Tm versus x for CxSi1x. The open and solid circles show the experimental data. The solid line represents the result of Vegard law between diamond and Si 1.0

Cp (J/g K)

0.8 0.6 0.4

3C-SiC

0.2

Cx Si 1-x

0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.11 Specific heat Cp versus x for CxSi1x at 300 K. The open and solid circles show the experimental data. The dashed line shows the linear interpolation result given by Equation (2.6), while the solid line is calculated from Equation (2.7)

The linear interpolation is concluded to estimate generally acceptable alloy Cp values. The solid line in Figure 2.11 shows the result of quadratic fit (in J/g K) Cp ðxÞ ¼ 0:713 þ 0:051x0:245x2

ð2:7Þ

2.2.2 III–V Semiconductor Alloy Sirota et al. [27] determined the Cp and Cv values of InPxAs1x from 5 to 160 K and their Cp data obtained at 160 K are shown graphically in Figure 2.12. The solid line shows the linear interpolation result between InP and InAs (in J/g K) Cp ðxÞ ¼ 0:220 þ 0:027x The linear interpolation scheme is found to yield generally acceptable alloy values.

ð2:8Þ

THERMAL PROPERTIES

55

0.26 In Px As 1-x Cp (J/g K)

0.24

0.22 T=160 K 0.20

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.12 Specific heat Cp versus x for InPxAs1x at 160 K. The experimental data are taken from Sirota et al. [27]. The solid line shows the linear interpolation result between the endpoint binary data

Sirota et al. [28] measured the Cp and Cv values of (GaAs)x(InP)1x quaternary from 5 to 300 K. Figure 2.13 shows the Cp data measured at 300 K. The solid line represents the result of linear interpolation given by (in J/g K) Cp ðxÞ ¼ 0:309 þ 0:014x

ð2:9Þ

0.34

Cp (J/g K)

0.32

0.30 (GaAs)x(InP)1-x 0.28

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.13 Specific heat Cp versus GaAs composition x for (GaAs)x(InP)1x at 300 K. The experimental data are taken from Sirota et al. [28]. The solid line shows the linear interpolation result between the endpoint binary data

It should be noted that the GaAs and InP values of 0.323 and 0.309 J/g K reported by Sirota et al. [28] are slightly smaller than those listed in Table 2.1. It can be seen in Figure 2.13, however, that the linear interpolation scheme is a useful tool for estimating alloy Cp values. Using the linear interpolation scheme, we obtain Cp versus x (0 x 1.0) and T (300 T 1500 K) for AlxGa1xAs as (Cp in J/g K) [29] Cp ðx; TÞ ¼ ð0:343 þ 0:133xÞ þ ð4:7 þ 1:5xÞ 105 Tð3:2 þ 3:3xÞ 103 T 2

ð2:10Þ

56

PROPERTIES OF SEMICONDUCTOR ALLOYS

2.2.3 II–VI Semiconductor Alloy The specific heat of CdxHg1xTe was measured from 5 to 300 K by Sirota et al. [30] and from room temperature up to 523 K by Gambino et al. [31]. The data of Gambino et al. revealed a remarkable anomaly in the form of an abrupt increase below a ‘step temperature’ which depended on x, as shown in Figure 2.14(a). The step temperature reached a maximum at about mid-range composition. It clearly signified an equilibrium solid-state phase change, which they suggested, could be a miscibility gap. As plotted in Figure 2.14(b), this phase change reaches 358 K at x ¼ 0.253 and might reach 240 K at x ¼ 0.2. Maleki and Holland [32] subjected Gambino’s data to a polynomial fit and summarized their results in tabular form. Sirota et al. [30] mentioned ‘an anomaly’ which caused their data to scatter from 15 to 80 K, but did not observe the phase boundary reported by Gambino et al., possibly because their temperatures were too low [32]. 0.23 x=1.0

0.21

x=0.8

440

(b)

400

Miscibility gap

360 0.20

0

x=0.6

0.19 0.18 0.17

x=0.5 x= 0.253 x=0

Cp (J/g K)

Cp (J/g K)

T (K)

0.22

480 CdxHg1-xTe

(a) 0.16 300 350 400 450 500 550 T(°C)

0.2 0.4 0.6 0.8 1.0 x

0.22 (c) 0.20 0.18 0.16 0

T=500 K

0.2 0.4 0.6 0.8 1.0 x

Figure 2.14 (a) Specific heat Cp versus temperature T for CdxHg1xTe with x ¼ 0 1.0. (b) Miscibility gap versus x for CdxHg1xTe. (c) Specific heat Cp versus x for CdxHg1xTe at 500 K. The experimental data in (a)–(c) were obtained from Gambino et al. [31]. The solid line in (c) shows the linear interpolation result between the endpoint binary data

The Cp versus x data for CdxHg1xTe measured at 500 K by Gambino et al. [31] are shown in Figure 2.14(c). The solid line represents the linear interpolation between CdTe and HgTe. It is understood that Cp can be successfully estimated from the linear interpolation scheme; however, a shallow dip in the experimental Cp–x plots is observed in the region centered at x 0.5. Gambino et al. [31] considered that the dip in Cp at x 0.5 is due to the presence of two phases and to the thermal effect associated with the change in equilibrium (solid $ solid(1) þ solid(2)) during Cp measurement, i.e. sample heating.

2.3 DEBYE TEMPERATURE 2.3.1 General Considerations Principally, the X-ray Debye temperature uD for pure metal can be given by [33] mu2D ¼

9f h2 CkB2 a

ð2:11Þ

THERMAL PROPERTIES

57

where m is the displacement of an atom from its lattice site, f is an average nearest-neighbor force constant, C is a numeric constant which depends on the lattice structure, kB is Boltzmann’s constant and a is the atomic mass unit. For a random alloy, the Debye temperature can be simply written as [33] mu2D ¼

X

xi mi u2Di þ

i

1X Aij xi xj ðmi u2Di þ mj u2Dj Þ 2 i„j

ð2:12Þ

where Aij is the factor accounting for the effect of an alloy disorder on the nearest-neighbor force constant. Although Equation (2.12) is for X-ray Debye temperature, it can also be applied to specificheat Debye temperatures since the two differ by a factor depending on Poisson’s ratio, which does not vary significantly from metal to metal and also from semiconductor to semiconductor [25]. If mi is not dependent on material and Aij is negligibly small, Equation (2.12) can then be simply written as u2D ðxÞ ¼

X

xi u2Di

ð2:13Þ

xi uDi

ð2:14Þ

i

The simplest Vegard law can be expressed as uD ðxÞ ¼

X i

2.3.2 Group-IV Semiconductor Alloy Figure 2.15 shows the Debye temperature uD versus x for CxSi1x at 300 K. The open and solid circles represent the experimental data for diamond, Si and 3C-SiC (x ¼ 0.5). The light solid line is calculated from Equation (2.13), while the dashed line is obtained from Equation (2.14).

2000 Cx Si 1- x

θ D (K)

1500

1000 3C-SiC

500

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.15 Debye temperature uD versus x for CxSi1x at 300 K. The heavy solid, light solid and dashed lines are calculated from Equations (2.12), (2.13) and (2.14), respectively

58

PROPERTIES OF SEMICONDUCTOR ALLOYS

The heavy solid line can also be obtained from Equation (2.12) with m ¼ mi(¼mj) ¼ 1 and Aij ¼ 1.4 (all these quantities are assumed to be non-dimensional). The high Debye temperature reflects low atomic mass and therefore short interatomic bond length in ANB8N semiconductors [25].

2.3.3 III–V Semiconductor Alloy The specific-heat Debye temperature uD for (a) InPxAs1x at 160 K and (b) (GaAs)x(InP)1x at 300 K is shown in Figure 2.16. The experimental data are taken from Sirota et al. [27,28]. The solid lines show the calculated results obtained using Equation (2.14). It was found that the uD versus x data can be satisfactorily explained by this expression. The Debye temperatures for these alloys are also found to vary with temperature in the same way as for the endpoint binaries, passing through a deep minimum in the region 10–20 K [27,28]. 450

θ D (K)

400

T=160 K

350 (a) InPx As1-x

300 250 600

θ D (K)

500

T=300 K

400 300 200

(b) (GaAs)x (InP) 1-x 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.16 Debye temperature uD versus x for (a) InPxAs1x at 160 K and (b) (GaAs)x(InP)1x at 300 K. The experimental data for InPxAs1x are taken from Sirota et al. [27] and for (GaAs)x(InP)1x from Sirota et al. [28]. The solid lines show the results calculated using Equation (2.14)

2.3.4 II–VI Semiconductor Alloy Nikiforov and Sredin [34] determined the specific-heat Debye temperature uD for CdxHg1xTe using a calorimeter. These results are shown in Figure 2.17. The solid line represents the linear interpolation result between the endpoint data in Table 2.1. As in the case of the III–V semiconductor alloys, the Debye temperature of CdxHg1xTe is a smooth and monotonic function of x; however, we can see an abrupt change at x ¼ 0.2. This may be due to an experimental error or may be the effect of any difference in crystalline quality. Since the Debye temperature is a model parameter that cannot be measured directly, it may contain considerable uncertainty, including numeric error.

THERMAL PROPERTIES

59

190 Cd x Hg1-xTe

θ D (K)

180 170 160 150 140 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.17 Debye temperature uD versus x for CdxHg1xTe at 300 K. The experimental data are taken from Nikiforov and Sredin [34]. The solid line shows the linear interpolation result using Equation (2.14) between the endpoint binary data

2.4 THERMAL EXPANSION COEFFICIENT 2.4.1 Group-IV Semiconductor Alloy During cooling down in epitaxial growth, a difference in thermal expansion can produce the driving force that moves the defects in the semiconductor heterostructure. Knowledge of the thermal expansion coefficient is, thus, essential not only from a physical point of view, but also for semiconductor device engineering. Figure 2.18 shows the linear thermal expansion coefficient ath for CxSi1x at 300 K. The experimental data are shown by the open and solid circles. The dashed line represents the 6 CxSi1-x 3C-SiC

4

-6

-1

α th (10 K )

5

3 2 1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.18 Linear thermal expansion coefficient ath versus x for CxSi1x at 300 K. The dashed line represents the linearly interpolated result of Equation (2.15). The solid line shows the quadratic fit of Equation (2.16)

60

PROPERTIES OF SEMICONDUCTOR ALLOYS

linear interpolation between diamond and Si (in 106 K1) ath ðxÞ ¼ 2:621:57x

ð2:15Þ

3C-SiC can be regarded as an alloy of C and Si (x ¼ 0.5); however, the linearly interpolated x ¼ 0.5 value in Figure 2.18 does not show good agreement with the experimental 3C-SiC data. It should be noted that C and Si crystallize in the diamond structure, but 3C-SiC crystallizes in the zinc-blende structure. The solid line in Figure 2.18 represents the quadratic fit (in 106 K1) ath ðxÞ ¼ 2:62 þ 2:03x3:60x2

ð2:16Þ

The ath value for SixGe1x was measured by Zhdanova et al. [35] and their results obtained at temperatures between 473 and 773 K are reproduced in Figure 2.19. The expansion decreased monotonically from Ge to Si. A gradual increase in ath was also found with increasing temperature from 300 K up to 1100 K. In Figure 2.19, there is a sudden change in the slope at x 0.15, which coincides with the transition of electronic properties from Ge-like to Si-like (Figure 6.8).

Figure 2.19 Linear thermal expansion coefficient ath versus x for SixGe1x at 473 and 773 K. [Reprinted from Izv. Akad. Nauk. SSSR Neorg. Mater. 3, 1263 (1967)]

The linear expansion coefficient ath is proportional to the specific heat Cv (Gr€uneisen rule) [25] 1 qa gCv Co ath ¼ ¼ a qT p 3V

ð2:17Þ

THERMAL PROPERTIES

61

where g is the averaged Gr€ uneisen parameter, Cv is the specific heat at constant volume, Co is the isothermal compressibility and V is the volume of the crystal. Theoretical work on ath, g and Cv was carried out by Kagaya et al. [26]. A simplified model was used where the lattice vibrations of Si and Ge atoms in the Si–Ge solid solution were assumed to be those of pure Si and Ge except that the lattice constant of the alloy was used. As in pure Si and Ge, the negative thermal expansion was predicted at low temperatures in SixGe1x.

2.4.2 III–V Semiconductor Alloy Figure 2.20 shows the x dependence of ath for AlxGa1xAs at 300 K. The experimental data are taken from Takahashi [36] and Bak-Misiuk [37]. The result of linear interpolation between AlAs and GaAs is shown by the solid line. The difference in ath between the GaAs substrate and the AlxGa1xAs epilayer can be approximated in Figure 2.20 by (in K1) Dath ðxÞ ¼ 1:75x 106

ð2:18Þ

8 AlxGa1-xAs

6

α th (10

-6

-1

K )

7

5 4 3

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.20 Linear thermal expansion coefficient ath versus x for AlxGa1xAs at 300 K. The experimental data are taken from Takahashi [36] and Bak-Misiuk et al. [37] (open circles). The linear interpolation result between the AlAs and GaAs values is shown by the solid line

The linear thermal expansion coefficients ath plotted against x for GaxIn1xP and GaPxAs1x at 300 K are shown in Figures 2.21(a) and 2.21(b), respectively. The experimental data are taken for GaxIn1xP from Kudman and Paff [38] and Leszczynski et al. [39] and for GaPxAs1x from Straumanis et al. [40]. It is apparent from Figure 2.21(a) that the thermal expansion of GaxIn1xP by Kudman and Paff [38] can be expressed as a linear function of x (solid circles). However, the endpoint values extrapolated from these data seem to be considerably larger than the generally accepted values (Table 2.1). Leszczynski et al. [39] measured the ath value of relaxed Ga0.5In0.5P layers grown on GaAs by LPE and reported it as 4.6 106 K1. This value (open circle) agrees well with the linear interpolation scheme (solid line). The data in Figure 2.21(b) can be approximated by the linear interpolation scheme (solid line). The experimental data can be read more exactly from the dashed curve written as (in 106 K1) ath ðxÞ ¼ 6:033:14x þ 2:00x2

ð2:19Þ

PROPERTIES OF SEMICONDUCTOR ALLOYS 7

7

6

6

5

5

α th (10-6 K-1)

α th (10-6 K-1)

62

4 GaxIn1-xP

3

4

2

2

1 0

GaPxAs1-x

3

1

(a) 0

0.2

0.4

0.6

0.8

0

1.0

(b) 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 2.21 Linear thermal expansion coefficients ath as a function of x for (a) GaxIn1xP and (b) GaPxAs1x at 300 K. The experimental data in (a) are taken from Kudman and Paff [38] (solid circles) and Leszczynski et al. [39] (open circle) and in (b) from Straumanis et al. [40] (open squares). The solid lines in (a) and (b) show the linear interpolation results between the endpoint binary data. The dashed line in (b) represents the result calculated using Equation (2.19)

The x dependence of ath for GaxIn1xPyAs1y has been investigated by many authors (see Adachi [41]). The experimental ath versus y for GaxIn1xPyAs1y/InP at 300 K is plotted in Figure 2.22 [41]. The ath values are found to almost linearly decrease with increasing y. The endpoint binary data are available for GaP, GaAs and InP, but not for InAs (Table 2.1). The solid line in Figure 2.22 represents the linear interpolation expression (in 106 K1) ath ðxÞ ¼ 4:89xy þ 6:03xð1yÞ þ 4:56ð1xÞy þ 5:50ð1xÞð1yÞ

ð2:20Þ

6.0 5.8

GaxIn1-xPyAs1-y / InP

-1

5.4

-6

α th (10 K )

5.6

5.2 5.0 4.8 4.6 4.4 0

0.2

0.4

0.6

0.8

1.0

y

Figure 2.22 Linear thermal expansion coefficients ath versus y for GaxIn1xPyAs1y/InP at 300 K. The experimental data are taken from Adachi [41]. The solid line represents the linear interpolation result of Equation (2.20)

THERMAL PROPERTIES

63

In obtaining Equation (2.20), we assumed the InAs value to be ath ¼ 5.50 106 K1. The linear interpolation expression in Figure 2.22 explains the experimental data satisfactorily. The ath value for AlxGa1xP has also been reported by Bessolov et al. [42].

2.4.3 II–VI Semiconductor Alloy The ath variations in ZnxHg1xTe and CdxHg1xTe have been measured from 4 to 290 K [43]. The bulk crystals were grown by the THM. The negative thermal expansions at temperatures below 65 K were clearly observed in ZnTe, CdTe and HgTe binaries and also in their alloys. The solid circles and triangles in Figure 2.23 show the experimental data measured at 280 K [43]. They are largely scattered. This is especially true for ZnxHg1xTe. 10

α th (10-6 K-1)

9 ZnxHg1-xTe

8 7 6

CdxHg1-xTe

5 4 3

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.23 Linear thermal expansion coefficients ath as a function of x for ZnxHg1xTe and CdxHg1xTe at 280 K. The experimental data are taken from Bagot et al. [43]. The solid lines represent the linear interpolation results between the endpoint binary data

The thermal expansion behaviors were also studied for ZnS0.03Se0.97 from 300 to 550 K [44] and for MgxZn1xSe (0.1 x 0.5) from 10 to 300 K [45]. The negative thermal expansion in conjunction with abnormal temperature dependence of the E0 edge was observed at T 75 K for MgxZn1xSe [45].

2.5 THERMAL CONDUCTIVITY AND DIFFUSIVITY 2.5.1 Thermal Conductivity (a) General considerations An exact calculation of the lattice thermal conductivity K is possible in principle, but lack of knowledge of various material parameters and the difficulty of obtaining an exact solution of phonon– phonon interactions are formidable barriers. In the case of semiconductor alloys, an additional contribution, which is the result of a random distribution of constituent atoms in sublattice sites, should be taken into consideration. A phenomenological model of the lattice thermal conductivity for semiconductor alloys was first proposed by Abeles [46]. His model 2 starts from three kinds of relaxation times: t 1 N ¼ B1 v (three-phonon normal process), 1 2 1 t U ¼ B2 v (three-phonon Umklapp process) and t D ¼ AGv2 (strain and mass point defects),

64

PROPERTIES OF SEMICONDUCTOR ALLOYS

where v is the phonon frequency, B1, B2 and A are constants independent of v and G is the disorder parameter depending on the masses and radii of the constituent atoms. The lattice thermal resistivity W ¼ K1 obtained by Abeles [46] is given by WðxÞ ¼ Wp ðxÞ

)1 ( 1 5 tan U ½1ðtan1 U=UÞ2 þ 1þ a ð2:21Þ 9 U ½ð1 þ aÞ=5aU 4 ð1=3ÞU 2 ðtan1 U=UÞ þ 1

with 1 5 UðxÞ2 ¼ U0 ðxÞ2 1 þ a 9

ð2:22Þ

U0 ðxÞ2 ¼ A1 GðxÞWp ðxÞ1

ð2:23Þ

where

In Equations (2.21)–(2.23), Wp(x) is the lattice thermal resistivity of the crystal in which the disorder lattice is replaced by an ordered virtual crystal, a is a normal/Umklapp ratio (a ¼ B1/B2) and A1 is nearly constant within a group of ANB8N semiconductors. G(x) can be written as ( GðxÞ ¼ xð1xÞ

DM MðxÞ

2

" þ«

Dd

#)

dðxÞ2

ð2:24Þ

where DM ¼ MA MB, Dd ¼ dA dB, M(x) ¼ xMA þ (1 x)MB and d(x) ¼ xdA þ (1 x)dB (Mi and di (i ¼ A, B) are the masses and radii of the constituent atoms). « is regarded as a phenomenological, adjustable parameter. The first and second terms in the curly brackets in Equation (2.24) correspond to the contributions from the mass-defect and strain scatterings, respectively. Abeles’s model was used by Adachi [47,48] and Nakwaski [49] for several III–V alloys. Adachi [47] showed that for an AxB1xC alloy WðxÞ ¼ xWAC þ ð1xÞWBC þ xð1xÞCAB

ð2:25Þ

is essentially the same as Equation (2.21), where WAC and WBC are the binary thermal resistivities and CAB is a contribution arising from the lattice disorder (G) due to the random distribution of A and B atoms in the cation sublattice sites. Equation (2.25) is known as the Nordheim rule [50,51] and can be readily converted to the lattice thermal conductivity K KðxÞ ¼

1 1 ¼ WðxÞ xWAC þ ð1xÞWBC þ xð1xÞCAB

ð2:26Þ

In an AxB1xCyD1y quaternary alloy, not only should the A–B disorder due to the random distribution of the A and B atoms in the cation sublattice and the C–D disorder due to the random distribution of the C and D atoms in the anionic sublattice be taken into consideration, but also the fact that both the cation and anion sublattices are disordered as well. Neglecting the

THERMAL PROPERTIES

65

cation–anion interaction effect, we obtain Kðx;yÞ ¼ ¼

1 Wðx;yÞ

1 xyWAC þxð1yÞWAD þð1xÞyWBC þð1xÞð1yÞWBD þxð1xÞCAB þyð1yÞCCD ð2:27Þ

In doped semiconductors, the thermal conductivity can be given by the sum of the lattice and electronic contributions. In a metal, the electronic thermal conductivity K and electrical conductivity s at temperature T are related by the Wiedemann–Franz law K ¼ LTs

ð2:28Þ

r ¼ LTW

ð2:29Þ

or, equivalently

where L is the Lorenz number and r is the electrical resistivity. The thermal resistivity W as a function of x for CuxAu1x is shown in Figure 2.24. Cu–Au alloy is among the best studied of all metallic alloy systems. The solid and open circles represent the experimental data for the ordered (CuAu and Cu3Au) and disordered phases, 3 CuxAu1-x

W (cm K / W)

2

1

Cu3Au

CuAu 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.24 Thermal resistivity W as a function of x for CuxAu1x at 300 K. The solid circles represent the experimental data obtained from ordered alloys (CuAu and Cu3Au), while the open circles represent the data taken from disordered alloys. The solid and dashed lines are calculated from Equation (2.25) with CCuAu ¼ 8.15 cm K/W and with and without properly taking into account the alloy ordering effect at x ¼ 0.5 and 0.75 (CuAu and Cu3Au), respectively

66

PROPERTIES OF SEMICONDUCTOR ALLOYS

respectively. These data were obtained from various sources (e.g. Jacobsson and Sundqvist [52]). The solid and dashed lines are calculated from Equation (A.5) (Equation (2.25)) with CCuAu ¼ 8.15 cm K/W and with and without properly taking into account the ordering effect at x ¼ 0.5 and 0.75 (CuAu and Cu3Au), respectively. It is evident from Figure 2.24 that the ordered alloy data are much smaller than those estimated from Equation (2.25) (dashed line). The ordering in metallic alloy is, thus, found to greatly decrease W, irrespective of the ordered structure (CuAu ¼ L10 (tetragonal) or Cu3Au ¼ L12 (cubic)). Similarly, the electrical resistivity r of the ordered phase is much lower than that of the disordered phases (Figure 12.1). The ordering effect in semiconductor alloys was observed to occur spontaneously during epitaxial growth [53]. Kuan et al. [54] first observed an ordered phase (CuAu-I type) in an MOCVD-grown AlGaAs epilayer. Since the first finding of CuPt-type ordering in SiGe alloy [55], this type of ordering and others have also been reported in many III–V and II–VI semiconductor alloys (Section 1.3.2). However, no clear ordering effect on the carrier transport properties in semiconductor alloys has been observed. In the following, therefore, we pay no attention to the spontaneous ordering effect, except for CxSi1x with x ¼ 0.5 (3C-SiC). Since the lifetimes of the dominant phonons in semiconductor alloys are 100 ps, the frequency dependence of K would not be observable in experiments unless f > 1 GHz. However, the frequency-dependent K of Si0.4Ge0.6, Ga0.51In0.49P and Ga0.47In0.53As was clearly observed over a wide range of modulation frequencies 0.1 < f < 10 MHz and temperatures 88 < T < 300 K from time-dependent TR measurements [56]. The reduction in K at high frequencies was consistent with a model calculation assuming that phonons with mean free paths larger than the thermal penetration depth do not contribute to K as measured in the experiment. (b) Group-IV semiconductor alloy There has been no experimental or theoretical work on the thermal conductivity of CxSi1x. This is because of the low solubility of C in Si (6 106) [57]. In Figure 2.25 only the experimental K and W data for 3C-SiC (x ¼ 0.5) together with those for diamond and Si have been plotted [48]. Note that diamond and Si crystallize in the diamond structure, while 3C-SiC crystallizes in the zinc-blende structure. It is, therefore, considered that 3C-SiC is an ordered form of CxSi1x (x ¼ 0.5), or more succinctly, it is a compound, not an alloy. The solid lines in Figure 2.25 are calculated from Equations (2.25) and (2.26) without taking into account the contribution of alloy disorder (i.e. CCSi ¼ 0 cm K/W), while the dashed lines are obtained by assuming CCSi ¼ 15 cm K/W and properly taking into account the ordering effect at x ¼ 0.5. The diamond and Si values used in the calculation are taken from Table 2.2. In Figure 2.25, the thermal conductivity and resistivity of 3C-SiC can be satisfactorily interpreted by the linear interpolation scheme (CAB ¼ 0 cm K/W). It is also expected from Figure 2.25(b) that the alloying leads to a large increase in W due to increased disorder scattering (dashed line). Similarly, not only a large increase in W in doped Si [58,59], but also a decrease in W in isotopically enriched diamond [60–62] and Si [59,63] has been reported. Systematic work on the thermal conductivity of SixGe1x was carried out by Dismukes et al. [64] and the values they obtained for K and W are plotted in Figure 2.26. The solid lines represent the results calculated using Equations (2.25) and (2.26) with CSiGe ¼ 50 cm K/W [48]. The thermal resistivity markedly increased with alloying. The W value at x 0.5 is about 28 times as large as those of Si and Ge. Such a feature was motivated by desire to obtain increased performance for thermoelectric power conversion since the figure of merit for such a device

THERMAL PROPERTIES

67

Table 2.2 Room-temperature thermal conductivity K and resistivity W for some group-IV and III–V semiconductors, together with alloy disorder parameters Cab used in the calculation of K and W. d ¼ diamond; w ¼ wurtzite; zb ¼ zinc-blende Material

K (W/cm K)

W (cm K/W)

Cab (cm K/W)

Diamond (d) Si (d) Ge (d) AlN (w) AlP (zb) AlAs (zb) AlSb (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

22 1.56 0.60 3.19 0.90 0.91 0.57 1.95 0.77 0.45 0.36 0.45 0.68 0.30 0.175

0.045 0.64 1.67 0.31 1.1 1.10 1.75 0.51 1.30 2.22 2.78 2.22 1.47 3.3 5.71

CSiGe ¼ 50 CAlGa ¼ 32 CAlIn ¼ 15a CGaIn ¼ 72 CNP ¼ 36a CNAs ¼ 12a CNSb ¼ 10a CPAs ¼ 25 CPSb ¼ 16a CAsSb ¼ 91

a

Estimated from Equation (2.31)

25 K ( W/ cm K )

20

(a) CxSi1-x

15 3C -SiC

10 5 0 5

W (cm K / W)

4

(b)

3 2 1 0

3C -SiC 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.25 (a) Thermal conductivity K and (b) resistivity W versus x for CxSi1x at 300 K. The experimental data for diamond, Si and 3C-SiC (x ¼ 0.5) are taken from Table 2.2. The solid lines are calculated from Equations (2.25) and (2.26) without taking into account the contribution of alloy disorder (i.e. CCSi ¼ 0 cm K/W), while the dashed lines are obtained assuming CCSi ¼ 15 cm K/W and properly taking into account the alloy ordering effect at x ¼ 0.5 (3C-SiC). [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

68

PROPERTIES OF SEMICONDUCTOR ALLOYS

K (W/cm K)

2.0 1.5

(a)

SixGe1-x

1.0 0.5 0

W (cmK/W)

20 15

(b)

10 5 0

0

0.2

0.4

0.6

0.8

1

x

Figure 2.26 (a) Thermal conductivity K and (b) resistivity W versus x for SixGe1x at 300 K. The experimental data are taken from Dismukes et al. [64]. The solid lines are obtained from Equations (2.25) and (2.26) with CSiGe ¼ 50 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

application varies proportionally to W. One method of achieving a high value for W is by the use of a fine-grain SiGe technique, in which a decrease in thermal conductivity of up to 50% was attained by increasing grain-boundary scattering of phonons [65]. (c) III–V semiconductor alloy Figure 2.27 shows the thermal conductivity K versus x for (Al, Ga)–V ternaries: (a) wAlxGa1xN and (b) AlxGa1xAs [48]. The experimental data are taken for w-AlxGa1xN from Daly et al. [66] and Liu and Balandin [67] and for AlxGa1xAs from Afromowitz [68] and Pichardo et al. [69]. The solid lines represent the results calculated using Equation (2.26). The III–V binary data are taken from Table 2.2. The reduction in K from the binary value is much larger in w-AlxGa1xN than in AlxGa1xAs. However, these (Al, Ga)–V ternaries have the same disorder parameter CAlGa ¼ 32 cm K/W (solid lines). It was also found [66] that polycrystalline GaN has a thermal conductivity K, which is more than an order of magnitude lower than that of bulk GaN. It should be noted that the thermal conductivity K (or thermal resistivity W) is a quantity given by a second-rank symmetric tensor [25]. The wurtzite-type III–N semiconductors thus have two tensor components, K? and Kk. However, the difference between K? and Kk usually appears to be less than the experimental uncertainty at room temperature [70]. Figure 2.28 shows the thermal conductivity K versus x for (Ga, In)–V ternaries: (a) w-GaxIn1xN, (b) GaxIn1xAs and (c) GaxIn1xSb [48]. The experimental data in (a) are taken from Pantha et al. [71], in (b) from Abrahams et al. [72] and Arasly et al. [73] and in (c) from Magomedov et al. [74]. The solid lines in (a)–(c) represent the results calculated using Equation (2.26) with CGaIn ¼ 72 cm K/W. It should be noted that the InN value WInN ¼ 2.22 cm K/W used in the calculation corresponds to that for InN ceramics, not the bulk crystalline value. The dashed line in Figure 2.28(a) shows the result calculated using Equation (2.26) and a

THERMAL PROPERTIES 3. 5

69

1. 0 0. 9

(a) w-AlxGa1-xN

3. 0

(b) AlxGa1-xAs

0. 8

K (W/cm K )

2. 5

0. 7 0. 6

2. 0

0. 5 1. 5

0. 4 0. 3

1. 0

0. 2 0. 5 0

0. 1 0

0. 2

0. 4

0. 6

0. 8

1. 0

0

0

0. 2

0. 4

0. 6

0. 8

1. 0

x

x

Figure 2.27 Thermal conductivity K versus x for (Al, Ga)-based III–V ternaries at 300 K: (a) w-AlxGa1xN and (b) AlxGa1xAs. The experimental data in (a) are taken from Daly et al. [66] and Liu and Balandin [67] and in (b) from Afromowitz [68] and Pichardo et al. [69]. The solid lines are obtained from Equation (2.26) with CAlGa ¼ 32 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

2.5

0.5

0.5

K (W/cm K)

(a) w-GaxIn1-xN

(b) GaxIn1-xAs

(c) GaxIn1-xSb

2.0

0.4

0.4

1.5

0.3

0.3

1.0

0.2

0.2

0.5

0.1

0.1

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 2.28 Thermal conductivity K versus x for (Ga, In)-based III–V ternaries at 300 K: (a) w-GaxIn1xN, (b) GaxIn1xAs and (c) GaxIn1xSb. The experimental data in (a) are taken from Pantha et al. [71] (solid triangles), in (b) from Abrahams et al. [72] and Arasly et al. [73] (solid circles) and in (c) from Magomedov et al. [74] (solid circles). The solid lines in (a)–(c) are obtained from Equation (2.26) with CGaIn ¼ 72 cm K/W. The dashed line in (a) is also obtained from Equation (2.26) with a properly chosen value of WInN ¼ 0.5 cm K/W (open circle), instead of the ceramics InN value of WInN ¼ 2.22 cm K/W (solid line). [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

70

PROPERTIES OF SEMICONDUCTOR ALLOYS

properly chosen value of WInN ¼ 0.5 cm K/W, instead of the ceramics value WInN ¼ 2.22 cm K/W (solid line). The small WInN effect is remarkable only in the limited region x < 0.2. It is well known that dilute alloying of GaAs with InAs is a very effective technique for reducing the dislocation density of semiinsulating GaAs crystals grown by the liquidencapsulated Czochralski method. Ohmer et al. [75] studied the effect of the addition of a small quantity of InAs on the thermal properties of GaAs. They reported that for x ¼ 0.005 the thermal conductivity is reduced to 50% of the GaAs value. This region is in accordance with theory if the size difference is considered and combined coherently with the mass difference [76]. Values of K and W versus x for AlAsxSb1x are shown in Figures 2.29(a) and 2.29(b), respectively [48]. The experimental data are taken from Borca-Tasciuc et al. [77]. The solid lines are calculated from Equations (2.25) and (2.26) with CAsSb ¼ 91 cm K/W. The agreement between the calculated and experimental results was found to be very satisfactory. 1.0 K (W/cm K )

0.8

(a)

0.6

AlAsxSb1-x

0.4 0.2 0

W (cm K /W)

30 25

(b)

20 15 10 5 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.29 (a) Thermal conductivity K and (b) resistivity W versus x for AlAsxSb1x at 300 K. The experimental data are taken from Borca-Tasciuc et al. [77]. The solid lines are obtained from Equations (2.25) and (2.26) with CAsSb ¼ 91 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

The lattice thermal conductivity K versus x plots for III–(P, As) ternaries GaPxAs1x and InPxAs1x are shown in Figures 2.30(a) and 2.30(b), respectively [48]. The experimental data for GaPxAs1x are taken from Carlson et al. [78] and Maycock [79] and for InPxAs1x from Maycock [79] and Bowers et al. [80]. The solid lines represent the results calculated using Equation (2.26) with CPAs ¼ 25 cm K/W. The fit-determined disorder parameter CPAs ¼ 25 cm K/W is comparable to CAlGa ¼ 32 cm K/W, but much smaller than CGaIn ¼ 72 cm K/W and CAsSb ¼ 91 cm K/W. The K values of some III–V quaternaries are shown in Figure 2.31 [48]. The experimental data for AlxGa1xAsySb1y/GaSb are taken from Borca-Tasciuc et al. [77] and Both et al. [81], for GaxIn1xPyAs1y/InP from Both et al. [82] and for GaxIn1xAsySb1y/GaSb from Both et al. [81]. The theoretical curves in Figure 2.31 are obtained from Equation (2.27) with (a) CAlGa ¼ 32 cm K/W and CAsSb ¼ 91 cm K/W, (b) CGaIn ¼ 72 cm K/W and CPAs ¼ 25 cm K/W and

THERMAL PROPERTIES 1.0

1.0

K (W/cm K )

0.9

0.9

(a) GaPxAs1-x

0.8

0.8

0.7

0.7

0.6

0.6

0.5

0.5

0.4

0.4

0.3

0.3

0.2

0.2

0.1

0.1

0

71

0

0.2

0.4

0.6

0.8

1.0

0

(b) InPxAs1-x

0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 2.30 Thermal conductivity K versus x for (P, As)-based III–V ternaries at 300 K: (a) GaPxAs1x and (b) InPxAs1x. The experimental data in (a) are taken from Carlson et al. [78] and Maycock [79] and in (b) from Maycock [79] and Bowers et al. [80]. The solid lines are obtained from Equation (2.26) with CPAs ¼ 25 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

0.7

0.7

(a) AlxGa1-xAsySb1-y /GaSb

K (W/cm K)

0.6

0.7

(b) GaxIn1-xPyAs1-y /InP

0.6

0.5

0.5

0.5

0.4

0.4

0.4

0.3

0.3

0.3

0.2

0.2

0.2

0.1

0.1

0.1

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 y

(c) GaxIn1-xAsySb1-y /GaSb

0.6

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 2.31 Thermal conductivity K versus x or y for III–V quaternaries at 300 K: (a) AlxGa1xAsySb1y/GaSb, (b) GaxIn1xPyAs1y/InP and (c) GaxIn1xAsySb1y/GaSb. The experimental data for AlxGa1xAsySb1y/GaSb are taken from Borca-Tasciuc et al. [77] and Both et al. [81], for GaxIn1xPyAs1y/InP from Both et al. [82] and for GaxIn1xAsySb1y/GaSb from Both et al. [81]. The solid lines are calculated from Equation (2.27) with (a) CAlGa ¼ 32 cm K/W and CAsSb ¼ 91 cm K/W, (b) CGaIn ¼ 72 cm K/W and CPAs ¼ 25 cm K/W and (c) CGaIn ¼ 72 cm K/W and CAsSb ¼ 91 cm K/W. The dashed line in (c) represents the result calculated using Equation (2.27) with the introduction of the very small disorder parameters CGaIn ¼ 10 cm K/W and CAsSb ¼ 20 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

72

PROPERTIES OF SEMICONDUCTOR ALLOYS

(c) CGaIn ¼ 72 cm K/W and CAsSb ¼ 91 cm K/W. The disorder parameters Cab are obtained from the III–V ternary data analyses. The lattice-matching relationships between x and y are taken from Tables 1.9 and 1.10. The agreement between the experimental and calculated data in Figures 2.31(a) and 2.31(b) is very good and successfully explains the composition dependence of K in the alloys. It should be noted, however, that the calculation in Figure 2.31(c) produces a K value considerably lower than the experimental value. The input of very small Cab values into Equation (2.27) improves the fit very well; however, the endpoint ternary K value (InAs0.91Sb0.09) becomes very large and the binary K value (GaSb) very small, compared with the generally accepted values. The dashed line in Figure 2.31(c) shows an example of such a calculation. Putting CGaIn ¼ 10 cm K/W and CAsSb ¼ 20 cm K/W into Equation (2.27), we obtain K ¼ 0.30 W/cm K for x ¼ 0 (InAs0.91Sb0.09) and 0.25 W/cm K for x ¼ 1.0 (GaSb), which are far from the generally accepted values. If the endpoint K values and Cab are available, the lattice thermal conductivity and its dependence on alloy composition can easily be calculated from Equation (2.26) or Equation (2.27). At the limit of weak scattering, the disorder parameter G in Equation (2.24) can be simply written as X Mi M 2 G¼ ci ð2:30Þ M i where ci is the fractional concentration of the ith species, Mi is the atomic mass of the ith species is the average atomic mass. and M Figure 2.32 plots the obtained Cab values versus G [48]. It can be seen that Cab decreases with the increase in G. The solid line represents the least-squares fit of the III–V ternaries given by (Cab in cm K/W) Cab ¼

Cαβ (cm K / W)

102

G 7:7

0:90

ð2:31Þ

As-Sb Si-Ge

Ga-In

Al-Ga P-As Cu-Au

101

10-1 Γ

Figure 2.32 Cab versus G determined for some group-IV binary and III–V ternary alloys and metallic Cu–Au alloy at 300 K. The solid line represents the least-squares fit (III–V ternary data) using Equation (2.31). [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

THERMAL PROPERTIES

73

Using this expression, the unknown Cab value can be estimated. For example, G of the cationic disorder system i ¼( Al, In) in Equation (2.30) is 0.384. Introducing this value into Equation (2.31), we obtain CAlIn ¼ 15 cm K/W. Figure 2.33 shows the lattice thermal conductivity as a function of x for (a) GaxIn1xP and (b) GaAsxSb1x [48]. No experimental data are available for these alloys. The solid lines are calculated from Equation (2.26) with CGaIn ¼ 72 cm K/W in (a) and CAsSb ¼ 95 cm K/W in (b). As expected, the calculated K value markedly decreases with alloying and exhibits a minimum at x 0.5. 1. 0

0. 5

K (W/cm K)

(a) GaxIn1-xP

(b) GaAsxSb1-x

0. 8

0. 4

0. 6

0. 3

0. 4

0. 2

0. 2

0. 1

0

0 0

0. 2

0. 4

0. 6

0. 8

1. 0

0

0. 2

0. 4

x

0. 6

0. 8

1. 0

x

Figure 2.33 Thermal conductivity K versus x for some III–V ternaries at 300 K: (a) GaxIn1xP and (b) GaAsxSb1x. These values were estimated from Equation (2.26) with CGaIn ¼ 72 cm K/W (a) and CAsSb ¼ 95 cm K/W (b) (solid lines). The solid circles represent the experimental endpoint binary data. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

In an AxByCzD (ABxCyDz) quaternary alloy, the lattice thermal conductivity K can be written as Kðx; y; zÞ ¼

1 1 ¼ Wðx; y; zÞ xWAD þ yWBD þ zWCD þ xyCAB þ xzCAC þ yzCBC

ð2:32Þ

with xþyþz ¼ 1

or z ¼ 1xy

ð2:33Þ

Since the thermal conductivity or resistivity in Equation (2.32) is specified in terms of the alloy composition x, y and z only, K or W of a quaternary alloy with arbitrary composition can easily be calculated. For example, the thermal conductivity of AlxGayIn1xyN can be estimated from (in W/cm K) KAlGaInN ðx; y; zÞ ¼

1 3:19x þ 1:95y þ 0:45z þ 32xy þ 15xz þ 72yz

ð2:34Þ

74

PROPERTIES OF SEMICONDUCTOR ALLOYS

Similarly, the K values for (AlxGa1x)0.53In0.47P/GaAs and (AlxGa1x)0.48In0.52As/InP can be estimated, as shown in Figure 2.34 [48]. The disorder parameters Cab used are taken from Table 2.2. The lattice-matching relationships between x and y for these quaternaries are taken from Table 1.11. 0.30

0.30

K (W/cm K)

(AlxGa1-x)0.53In0.47P/GaAs

(AlxGa1-x)0.48In0.52As/InP

0.25

0.25

0.20

0.20

0.15

0.15

0.10

0.10

0.05

0.05 (a)

0

0

0.2

0.4

0.6 x

0.8

(b) 1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.34 Thermal conductivity K versus x for some III–V quaternaries at 300 K: (a) (AlxGa1x)0.53In0.47P/GaAs and (b) (AlxGa1x)0.48In0.52As/InP. These values were estimated from Equation (2.32) with CAlGa ¼ 32 cm K/W, CAlIn ¼ 15 cm K/W and CGaIn ¼ 72 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

(d) II–VI semiconductor alloy Ioffe and Ioffe [83] reported the thermal conductivity of ZnTe–CdTe, CdSe–HgSe, ZnSe–ZnTe, HgSe–HgTe, ZnSe–CdTe and ZnTe–CdSe alloys. Each of the starting materials was crushed into a fine powder, carefully blended in the required proportions, compressed under a pressure of 2–5 t/cm2 at a temperature of about 300 C and then repeatedly annealed at higher temperatures until a stable value of thermal conductivity was attained. All the experimental data showed a marked decrease in thermal conductivity with alloying. Because of the ceramic-like nature of the samples, their absolute values may be much smaller than those of the bulk crystalline materials. Aliev et al. [84] have reported the temperature dependence of K for CdxHg1xTe with x ¼ 00.2. These results are shown in Figure 2.35. The data give a maximum K near 8 K. In the temperature range from 10 to 100 K, HgTe (x ¼ 0) has a thermal conductivity proportional to T 1.2. The alloys with x > 0 have lower thermal conductivities and the temperature exponents are also less. The experimentally determined exponents for various non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Table 2.9 of Adachi [25]. The thermal conductivities K for ZnxHg1xTe and CdxHg1xTe and their melts were reported by Sha et al. [85] and Su [86], respectively. These data were determined from the experimental diffusivities and theoretical specific heats (Section 2.5.2).

THERMAL PROPERTIES

75

Figure 2.35 Thermal conductivity K for CdxHg1xTe with x ¼ 0, 0.05, 0.1 and 0.2. [Reprinted from Sov. Phys Solid State 2, 719 (1960)] The solid line represents the exponential relationship, K / T 1.2

2.5.2 Thermal Diffusivity (a) General considerations The thermal diffusivity D can be obtained from the thermal conductivity K by means of the definition D¼

K Cp g

ð2:35Þ

where Cp and g represent the specific heat at constant pressure and crystal density, respectively. Thermal diffusivity D is measured in cm2/s. (b) Alloy value Figure 2.36 shows the inverse plots of D versus x for (a) CxSi1x and (b) AlxGa1xAs. The endpoint data are indicated by the open circles. The experimental data for 3C-SiC is also shown in Figure 2.36(a) by the solid circle. The solid line in Figure 2.36(b) is obtained from Equation (2.35) using the K and Cp values in Table 2.2 (Equation (2.26)) and Equation (2.10), respectively. The inverse thermal diffusivity D1 of 3C-SiC is found to be well interpreted by the linear interpolation between the endpoint data. Figure 2.37 shows the plot of K and D versus x for (GaAs)x(InP)1x quaternary. The K values are obtained from (in W/cm K) KðGaAsÞðInPÞ ðxÞ ¼

1 2:22x þ 1:47ð1xÞ þ 72xð1xÞ þ 25xð1xÞ

ð2:36Þ

76

PROPERTIES OF SEMICONDUCTOR ALLOYS

D-1 (s/cm2)

1.5 1.2

(a) CxSi1-x

3C-SiC

0.9 0.6 0.3 0 20

D-1 (s/cm2)

16 12 8 (b) AlxGa1-xAs

4 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.36 Inverse thermal diffusivity D versus x for (a) CxSi1x and (b) AlxGa1xAs at 300 K. The solid line in (a) represents the linear interpolation result between the endpoint data (open circles)

K (W/cm K)

0.8 0.6

(a)

0.4 (GaAs)x(InP)1-x 0.2 0 0.5

D (cm2/s)

0.4

(b)

0.3 0.2 0.1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.37 (a) Thermal conductivity K and (b) diffusivity D versus x for (GaAs)x(InP)1x quaternary at 300 K. The solid circles represent the experimental endpoint binary data

The Cp values used in the calculation of D are taken from Equation (2.9), while g is interpolated between GaAs and InP.

REFERENCES [1] H. St€ohr and W. Klemm, Z. Anorg. Allg. Chem. 241, 305 (1939). [2] T. Soma, Phys. Status Solidi B 111, K23 (1982).

THERMAL PROPERTIES [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34] [35] [36] [37] [38] [39] [40] [41]

77

L. M. Foster and J. F. Woods, J. Electrochem. Soc. 118, 1175 (1971). G. B. Stringfellow, J. Phys. Chem. Solids 33, 665 (1972). M. B. Panish and M. Ilegems, Prog. Solid State Chem. 7, 39 (1972). S. Adachi, J. Appl. Phys. 58, R1 (1985). N. A. El-Masry, E. L. Piner, S. X. Liu, and S. M. Bedair, Appl. Phys. Lett. 72, 40 (1998). D. Doppalapudi, S. B. Basu, K. F. Ludwig, Jr., and T. D. Moustakas, J. Appl. Phys. 84, 1389 (1998). T. Saito and Y. Arakawa, Phys. Rev. B 60, 1701 (1999). T. Takeyama, M. Yuri, K. Itoh, T. Baba, and J. S. Harris, Jr., J. Appl. Phys. 88, 1104 (2000). L. K. Teles, J. Furthm€uller, L. M. R. Scolfaro, J. R. Leite, and F. Bechstedt, Phys. Rev. B 62, 2475 (2000). M. Ferhat and F. Bechstedt, Phys. Rev. B 65, 075213 (2002). J. Adhikari and D. A. Kofke, J. Appl. Phys. 95, 4500 (2004). S. Y. Karpov, N. I. Podolskaya, I. A. Zhmakin, and A. I. Zhmakin, Phys. Rev. B 70, 235203 (2004). C. K. Gan, Y. P. Feng, and D. J. Srolovitz, Phys. Rev. B 73, 235214 (2006). S. Raghavan, J. P. Hajra, G. N. K. Iyengar, and K. P. Abraham, Thermochim. Acta 189, 151 (1991). V. L. Solozhenko, A. N. Baraov, and V. Z. Turkevich, Solid State Commun. 138, 534 (2006). J. Steininger, A. J. Strauss, and R. F. Brebrick, J. Electrochem. Soc. 117, 1305 (1970). A. G. Fischer and W. H. Fonger, Report No. 3 (1965), Contract No. AF 19 (628)-3866, US Air Force, Cambridge Research Laboratories, Bedford, Mass., USA. A. J. Strauss and J. Steininger, J. Electrochem. Soc. 117, 1420 (1970). J. Steininger and A. J. Strauss, J. Cryst. Growth 13/14, 657 (1972). K. Ohata, J. Saraie, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1198 (1973). D. A. Wood, K. D. Rogers, D. W. Lane, G. J. Conibeer, and D. Parton, J. Mater. Sci. Lett. 17, 1511 (1998). See, T. C. Harman, in Physics and Chemistry of II–VI Compounds (edited by M. Aven and J. S. Prener), North-Holland, Amsterdam, 1967, p. 767. S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. H.-M. Kagaya, Y. Kitani, and T. Soma, Solid State Commun. 58, 399 (1986). A. N. N. Sirota, A. M. Antyukhov, and V. A. Fedorov, Sov. Phys. Dokl. 26, 701 (1981). A. N. N. Sirota, A. M. Antyukhov, V. V. Novikov, and A. A. Sidorov, Sov. Phys. Dokl. 27, 754 (1982). S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties. World Scientific, Singapore, 1994. N. N. Sirota, N. P. Gavaleshko, V. V. Novikova, A. V. Novikova, and V. M. Frasunyak, Russ. J. Phys. Chem. 64, 603 (1990). M. Gambino, V. Vassiliev, and J. P. Bros, J. Alloys Compounds 176, 304 (1987). H. Maleki and L. R. Holland, in Properties of Narrow Gap Cadmiun-based Compounds, EMIS Datareviews Series No. 10 (edited by P. Capper), INSPEC, London, 1994, p. 48. C. G. Shirley, Acta Crsyt. A 31, 853 (1975). V. N. Nikiforov and V. G. Sredin, Rus. Phys. J. 49, 337 (2006). V. V. Zhdanova, M. G. Kakna, and T. Z. Samadashvili, Izv. Akad. Nauk. SSSR Neorg. Mater. 3, 1263 (1967). N. S. Takahashi, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 3. _ J. Bak-Misiuk, J. Domagała, W. Paszkowicz, J. Trela, Z. R. Zytkiewicz, M. Leszczy nski, K. Reginski, J. Muszalski, J. H€artwig, and M. Ohler, Acta Phys. Polonica A 91, 911 (1997). I. Kudman and R. J. Paff, J. Appl. Phys. 43, 3760 (1972). M. Leszczynski, A. Kulik, and P. Ciepielewski, Phys. Status Solidi A 119, 495 (1990). M. E. Straumanis, J.-P. Krumme, and M. Rubenstein, J. Electrochem. Soc. 114, 640 (1967). S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992.

78

PROPERTIES OF SEMICONDUCTOR ALLOYS

[42] V. N. Bessolov, S. G. Konnikov, V. E. Umanskii, and Y. P. Yakoviev, Sov. Phys. Tech. Phys. 28, 257 (1983). [43] D. Bagot, R. Granger, and S. Rolland, Phys. Status Solidi B 177, 295 (1993). [44] J. R. Kim, R. M. Park, and K. S. Jones, Mater. Res. Soc. Symp. Proc. 340, 475 (1994). [45] W.-T. Kim, Phys. Rev. B 59, 4572 (1999). [46] B. Abeles, Phys. Rev. 131, 1906 (1963). [47] S. Adachi, J. Appl. Phys. 54, 1844 (1983). [48] S. Adachi, J. Appl. Phys. 102, 063502 (2007). [49] W. Nakwaski, J. Appl. Phys. 64, 159 (1988). [50] L. Nordheim, Ann. Phys. 401, 607 (1931). [51] L. Nordheim, Ann. Phys. 401, 641 (1931). [52] P. Jacobsson and B. Sundqvist, J. Phys. Chem. Solids 49, 441 (1988). [53] A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys, Kluwer Academic, New York, 2002. [54] T. S. Kuan, T. F. Kuech, W. I. Wang, and E. L. Wilkie, Phys. Rev. Lett. 54, 201 (1985). [55] A. Ourmazd and J. C. Bean, Phys. Rev. Lett. 55, 765 (1985). [56] Y. K. Koh and D. G. Cahill, Phys. Rev. B 76, 075207 (2007). [57] E. T. Croke, A. T. Hunter, C. C. Ahn, T. Laursen, D. Chandrasekhar, A. E. Bair, D. J. Smith, and J. W. Mayer, J. Cryst. Growth 175–176, 486 (1997). [58] M. Asheghi, K. Kurabayashi, R. Kasnavi, and K. E. Goodson, J. Appl. Phys. 91, 5079 (2002). [59] D. G. Cahill and F. Watanabe, Phys. Rev. B 70, 235322 (2004). [60] T. R. Anthony, W. F. Banholzer, J. F. Fleischer, L. Wei, P. K. Kuo, R. L. Thomas, and R. W. Pryor, Phys. Rev. B 42, 1104 (1990). [61] D. G. Onn, A. Witek, Y. Z. Wie, T. R. Anthony, and W. F. Banholzer, Phys. Rev. Lett. 68, 2806 (1992). [62] J. R. Olson, R. O. Pohl, J. W. Vandersande, A. Zoltan, T. R. Anthony, and W. F. Banholzer, Phys. Rev. B 47, 14850 (1993). [63] W. S. Capinski, H. J. Maris, E. Bauser, I. Silier, M. Asen-Palmer, T. Ruf, M. Cardona, and E. Gmelin, Appl. Phys. Lett. 71, 2109 (1997). [64] J. P. Dismukes, L. Ekstrom, E. F. Steigmeier, I. Kudman, and D. S. Beers, J. Appl. Phys. 35, 2899 (1964). [65] C. B. Vining, W. Laskow, J. O. Hanson, R. R. Van der Beck, and P. D. Gorsuch, J. Appl. Phys. 69, 4333 (1991). [66] B. C. Daly, H. J. Maris, A. V. Nurmikko, M. Kuball, and J. Han, J. Appl. Phys. 92, 3820 (2002). [67] W. Liu and A. A. Balandin, Appl. Phys. Lett. 85, 5230 (2004). [68] M. A. Afromowitz, J. Appl. Phys. 44, 1292 (1973). [69] J. L. Pichardo, J. J. Alvarado-Gil, A. Cruz, J. G. Mendoza, and G. Torres, J. Appl. Phys. 87, 7740 (2000). [70] G. A. Slack and S. B. Austerman, J. Appl. Phys. 42, 4713 (1971). [71] B. N. Pantha, R. Dahal, J. Li, J. Y. Lin, H. X. Jiang, and G. Pomrenko, Appl. Phys. Lett. 92, 042112 (2008). [72] M. S. Abrahams, R. Braunstein, and F. D. Rosi, J. Phys. Chem. Solids 10, 204 (1959). [73] D. G. Arasly, R. N. Ragimov, and M. I. Aliev, Sov. Phys. Semicond. 24, 225 (1990). [74] Y. B. Magomedov, N. L. Kramynina, and S. M. Ismaılov, Sov. Phys. Solid State 34, 1486 (1992). [75] M. C. Ohmer, W. C. Mitchel, G. A. Graves, D. E. Holmes, H. Kuwamoto, and P. W. Yu, J. Appl. Phys. 64, 2775 (1988). [76] F. Szmulowicz, F. L. Madarasz, P. G. Klemens, and J. Diller, J. Appl. Phys. 66, 252 (1989). [77] T. Borca-Tasciuc, D. W. Song, J. R. Meyer, I. Vurgaftman, M.-J. Yang, B. Z. Nosho, L. J. Whitman, H. Lee, R. U. Martinelli, G. W. Turner, M. J. Manfra, and G. Chen, J. Appl. Phys. 92, 4994 (2002). [78] R. O. Carlson, G. A. Slack, and S. J. Silverman, J. Appl. Phys. 36, 505 (1965). [79] P. D. Maycock, Solid-State Electron. 10, 161 (1967). [80] R. Bowers, J. E. Bauerle, and A. J. Cornish, J. Appl. Phys. 30, 1050 (1959).

THERMAL PROPERTIES [81] [82] [83] [84] [85] [86]

79

W. Both, A. E. Bochkarev, A. E. Drakin, and B. N. Sverdlov, Cryst. Res. Technol. 24, K161 (1989). W. Both, V. Gottschalch, and G. Wagner, Cryst. Res. Technol. 21, K85 (1986). A. V. Ioffe and A. F. Ioffe, Sov. Phys. Solid State 2, 719 (1960). S. A. Aliev, T. G. Gadzhive, and R. I. Selim-zade, Sov. Phys. Solid State 31, 346 (1989). Y.-G. Sha, C.-H. Su, K. Mazuruk, and S. L. Lehoczky, J. Appl. Phys. 80, 752 (1996). C.-H. Su, J. Cryst. Growth 78, 51 (1986).

3 Elastic Properties 3.1 ELASTIC CONSTANT 3.1.1 General Considerations The second-order elastic stiffness [C] and compliance tensors [S] are defined by the generalized Hooke’s law: ½X ¼ ½C½e or ½e ¼ ½S½X, where [X] and [e] are, respectively, the elastic stress and strain tensors which have six components. The elastic tensors [C] and [S] are second-order fourth-rank and have symmetric 6 6 components. Their explicit tensor forms are given in Adachi [1]. We present in Tables 3.1–3.3 the elastic stiffness and compliance constants for a number of group-IV, III–V and II–VI semiconductors used for obtaining alloy values.

3.1.2 Room-temperature Value (a) Group-IV semiconductor alloy Figure 3.1 shows the elastic constants Cij of the metallic alloy Cu–Au. The solid and open circles represent the experimental ordered (CuAu3 and Cu3Au) and disordered phase data, respectively, gathered from various sources. The solid lines show the linear interpolation values between Au and Cu. No clear ordering effect can be found in the elastic properties of the metallic alloy. Figure 3.2 shows the plots of experimental Cij data for 3C-SiC (x ¼ 0.5), together with those for diamond and Si. Note that 3C-SiC crystallizes in the zinc-blende structure and is a compound, not an alloy. The solid lines show the linear interpolation between diamond and Si. Because of the extremely large Cij values of diamond, the linearly interpolated SiC values deviate considerably from the experimental values. Mendik et al. [2] determined the elastic constants of a relaxed Si0.49Ge0.51 film using Brillouin scattering and his data are shown in Figure 3.3, together with those of Si and Ge. The alloy value can be safely estimated using the linear interpolation scheme. (b) III–V semiconductor alloy Only a few reports of the direct measurement of elastic constants are available for III–V semiconductor alloys. The elastic constants Cij of GaxIn1xSb have been determined using a pulse echo method [3]. Figure 3.4 shows these results. The linearly interpolated values are shown by the solid lines and the experimental data are in good agreement with the linear interpolation results. Figure 3.5 shows the elastic constants Cij versus y or x for (a) GaxIn1xPyAs1y/InP and (b) (AlxGa1x)0.53In0.47P/GaAs. The solid circles show the endpoint data determined by Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

82

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 3.1 Elastic stiffness Cij and compliance constants Sij for a number of cubic group-IV, III–V and II–VI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

Cij (1011 dyn/cm2)

Material

Sij (1012 cm2/dyn)

C11

C12

C44

S11

S12

S44

107.9 16.564 12.870 6.90 39.0

12.4 6.394 4.770 2.93 14.2

57.8 7.951 6.670 3.62 25.6

0.0949 0.7691 0.9718 1.94 0.318

0.00978 0.2142 0.2628 0.578 0.085

0.1730 1.2577 1.499 2.76 0.391

IV

Diamond (d) Si (d) Ge (d) Sn (d)a 3C-SiC (zb)

III–V

BN (zb) BP (zb) BAs (zb)b AlN (zb)b AlP (zb)b AlAs (zb) AlSb (zb) GaN (zb)b GaP (zb) GaAs (zb) GaSb (zb) InN (zb)b InP (zb) InAs (zb) InSb (zb)

82.0 31.5 27.9 31.5 15.0 11.93 8.769 29.1 14.050 11.88 8.838 19.2 10.22 8.329 6.608

19.0 10 12.0 15.0 6.42 5.72 4.341 14.8 6.203 5.38 4.027 7.30 5.73 4.526 3.531

48.0 16 11.3 18.5 6.11 5.72 4.076 15.8 7.033 5.94 4.320 9.35 4.42 3.959 3.027

0.134 0.37 0.484 0.458 0.897 1.216 1.697 0.523 0.9756 1.173 1.583 0.659 1.639 1.945 2.410

0.025 0.09 0.145 0.148 0.269 0.394 0.5618 0.176 0.2988 0.366 0.4955 0.182 0.589 0.6847 0.8395

0.208 1.00 0.885 0.541 1.64 1.748 2.453 0.633 1.422 1.684 2.315 1.07 2.26 2.526 3.304

II–VI

BeS (zb)b BeSe (zb)b BeTe (zb)b MgO (rs) MgS (zb)b MgSe (zb)b MgTe (zb)b ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

12.3 11.0 8.87 29.4 8.88 7.58 5.28 10.2 8.57 7.15 7.70 6.67 5.35 8.13 6.08 5.32

7.30 6.66 5.54 9.3 5.53 4.86 3.66 6.46 5.07 4.08 5.39 4.63 3.69 6.22 4.46 3.68

5.69 5.03 3.86 15.5 3.87 3.17 1.93 4.46 4.05 3.11 2.36 2.23 2.02 2.64 2.23 2.08

1.47 1.66 2.16 0.401 2.16 2.64 4.38 1.95 2.09 2.39 3.07 3.48 4.27 3.65 4.34 4.33

0.55 0.63 0.83 0.096 0.83 1.03 1.79 0.76 0.78 0.85 1.26 1.42 1.74 1.58 1.84 1.77

1.76 1.99 2.59 0.647 2.58 3.15 5.18 2.25 2.47 3.25 4.24 4.48 4.95 3.79 4.49 4.80

a b

Obtained from an analysis of the phonon dispersion curves at 90 K Calculated or estimated

ELASTIC PROPERTIES

83

Table 3.2 Elastic stiffness constant Cij for a number of hexagonal group-IV, III–V and II–VI semiconductors at 300 K (in 1011 dyn/cm2). w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)) System

Material

C11

C12

IV

2H-SiC (w)b

50.1

11.1

III–V

BN (h) AlN (w) GaN (w) InN (w)

52.0 41.0 37.3 19.0

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

46.1 20.9 12.2 8.65 7.41

a b

C33

C44

C66a

5.2

55.3

16.3

19.5

43.1 14.0 14.1 10.4

37.0 10.0 8.0 12.1

42.4 39.0 38.7 18.2

6.5 12.0 9.4 0.99

4.5 13.5 11.6 4.3

12.6 12.0 5.8 5.40 4.52

8.85 10.4 4.2 4.73 3.9

49.2 21.8 13.8 9.44 8.43

14.8 4.41 2.87 1.50 1.34

16.8 4.45 3.2 1.63 1.45

C13

C66 ¼ 1/2(C11 C12) Assuming that the 2H-SiC values are the same as those for 6H-SiC within experimental error

Table 3.3 Elastic compliance constant Sij for a number of hexagonal group-IV, III–V and II–VI semiconductors at 300 K (in 1012 cm2/dyn). w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)) System

Material

IV

S12

S13

S33

2H-SiC (w)b

0.211

0.045

0.016

0.184

0.614

0.512

III–V

BN (h) AlN (w) GaN (w) InN (w)

0.726 0.285 0.320 0.957

0.398 0.085 0.112 0.206

0.286 0.051 0.043 0.499

0.735 0.283 0.276 1.21

1.54 0.833 1.06 10.1

2.25 0.740 0.864 2.33

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

0.240 0.782 1.10 2.08 2.32

0.060 0.345 0.45 1.00 1.12

0.032 0.210 0.20 0.54 0.55

0.215 0.664 0.86 1.60 1.69

0.677 2.24 3.48 6.66 7.47

0.600 2.254 3.10 6.16 6.88

a b

S44

S66a

S11

S66 ¼ 2(S11 S12) Assuming that the 2H-SiC values are the same as those for 6H-SiC within experimental error

Brillouin scattering for Ga0.47In0.53As [4] and Ga0.53In0.47P [5]. Since the lattice-matched quaternaries have thesame lattice constants over the entire composition range (aInP ¼ 5.8690 A or aGaAs ¼ 5.65330 A), their elastic constants are not expected to show strong dependence on the alloy composition [1]. The solid lines in Figures 3.5(a) and 3.5(b) represent the results calculated using Equations (A.6) and (A.8), respectively.

84

PROPERTIES OF SEMICONDUCTOR ALLOYS

C44 (GPa)

C12 (GPa)

C11 (GPa)

CuAu3 (LI2)

220 200 180 160 140 180 160 140 120 100 100 80 60 40 20 0

Cu3Au (LI2)

(a) Cux Au1-x (b)

(c) 0.2

0.4

x

0.6

0.8

1.0

Figure 3.1 Elastic constants Cij of Cu–Au. The solid and open circles represent the experimental ordered (LI2 type) and disordered alloy data, respectively. The solid lines show the linear interpolation results between Au and Cu

CxSi1-x (a)

C12 (GPa)

C11 (GPa)

1200 900 600 300 0 180 150 120 90 60 30 0 800 600 400 200 0 0

C44 (GPa)

3C-SiC

(b)

(c) 0.2

0.4

x

0.6

0.8

1.0

Figure 3.2 Elastic constants Cij of CxSi1x at 300 K. The solid circles represent the 3C-SiC data (x ¼ 0.5). The solid lines show the linear interpolation results between the endpoint elemental data

(c) II–VI semiconductor alloy The elastic constant C11 of MBE-BexZn1xSe on GaAs(100) has been determined using Brillouin scattering [6]. Figure 3.6 shows these results. The BeSe value is estimated from the simple Cij–a (lattice parameter) relationship described in Adachi [1]. The solid line is linearly interpolated between the endpoint binary data. The experimental data in Figure 3.6 suggest an upward bowing. Peiris et al. [6] determined C11 from the sound velocities vs by measuring

ELASTIC PROPERTIES

85

C11 (GPa)

180 150

SixGe1-x

120

(a)

C12 (GPa)

90 80 60 40

(b)

C44 (GPa)

20 100 80 60 40 0

(c) 0.2

0.4

x

0.6

0.8

1.0

Figure 3.3 Elastic constants Cij of SixGe1x at 300 K. The experimental data (x ¼ 0.49) are taken from Mendik et al. [2]. The solid lines show the linear interpolation results between the endpoint elemental data C11 (GPa)

90 80

GaxIn1-xSb

70

(a)

C44 (GPa)

C12 (GPa)

60 45 40 35 30 50 45 40 35 30 25

(b)

(c) 0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.4 Elastic constants Cij of GaxIn1xSb at 300 K. The experimental data are taken from Galibert and Bougnot [3]. The solid lines show the linear interpolation results between the endpoint binary data

frequency shift Dv of the Brillouin components using the relationship Dv ¼ 2vL n

vs u sin 2 c

ð3:1Þ

where vL is the frequency of the incident laser radiation, n is the refractive index of the material, c is the speed of light in vacuum and u is the scattering angle (180 ). Using a prism coupler technique, they also determined n for BexZn1xSe. Figure 3.7 shows the elastic constants Cij versus x for ZnxCd1xTe. The experimental data are taken from Andrusiv et al. [7] (x ¼ 0.35, 0.57 and 0.71), from Maheswaranathan et al. [8]

PROPERTIES OF SEMICONDUCTOR ALLOYS

C44 (GPa)

C12 (GPa)

C11 (GPa)

86

130 120 110 100 90 70

130 120 110 100 90 70

(a) GaxIn1-xPyAs1-y /InP

60

60

50

50

40 70

40 70

60

60

50

50

40

0

0.2

0.4

y

0.6

0.8

40

1.0

(b) (AlxGa1-x)0.53In0.47P/GaAs

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.5 Elastic constants Cij versus y or x for (a) GaxIn1xPyAs1y/InP and (b) (AlxGa1x)0.53 In0.47P/GaAs at 300 K. The open circles in (a) represent the InP data, while the solid circles in (a) and (b) show the endpoint ternary data taken from Carlotti et al. [4] (Ga0.47In0.53As) and Hassine et al. [5] (Ga0.53In0.47P), respectively. The solid lines show the linear interpolation results of Equations (A.6) and (A.8)

140

C11 (GPa)

120 100 80 60 0

Bex Zn1-xSe 0.2

0.4

x

0.6

0.8

1.0

Figure 3.6 Elastic constant C11 of MBE-grown BexZn1xSe on GaAs(1 0 0) at 300 K. The experimental data are taken from Peiris et al. [6]. The solid line shows the linear interpolation result between the endpoint binary data

(x ¼ 0.48) and from Queheillalt and Wadley [9] (x ¼ 0.04). These data are in agreement with the linearly interpolated values within experimental accuracy.

3.1.3 External Perturbation Effect (a) Temperature effect Only a few reports are available on the temperature dependence of Cij for III–V and II–VI alloys [3,7,9]. Figure 3.8 shows the linearly interpolated dCij/dT versus y for GaxIn1xPyAs1y/ InP calculated from Equation (A.6). The binary values used are taken from Table 3.8 in Adachi [1].

ELASTIC PROPERTIES

87

C11 (GPa)

80 ZnxCd1-xTe

70 60

(a)

C44 (GPa)

C12 (GPa)

50 45 40 35 30 35 30 25 20 15

(b)

(c) 0

0.2

0.4

x

0.6

0.8

1.0

dC11 /dT dC44 /dT dC12 /dT (107 dyn/cm2 K) (107 dyn/cm2 K) (107 dyn/cm2 K)

Figure 3.7 Elastic constants Cij versus x for ZnxCd1xTe at 300 K. The experimental data are taken from Andrusiv et al. [7] (x ¼ 0.35, 0.57 and 0.71), from Maheswaranathan et al. [8] (x ¼ 0.48) and from Queheillalt and Wadley [9] (x ¼ 0.04). The solid lines show the linear interpolation results between the endpoint binary data

-12 -14

GaxIn1-xPyAs1-y /InP

-16

(a)

-18 -4 (b)

-6 -8 -10 -2 -4 -6 -8 -10 0

(c) 0.2

0.4

y

0.6

0.8

1.0

Figure 3.8 Linearly interpolated dCij/dT versus y for GaxIn1xPyAs1y/InP at 300 K. The binary dCij/dT data used in the calculation (Equation (A.6)) are taken from Adachi [1]

The temperature-dependent Cij values of ZnxCd1xTe have been determined from 78 to 300 K [7] and from 300 up to 1413 K [9]. The solid circles in Figure 3.9 show the dCij/dT data for ZnxCd1xTe (x ¼ 0.04) [9]. The endpoint data taken from Table 3.8 in Adachi [1] are also shown by the open circles. The x ¼ 0.04 data are found to largely deviate from the linearly interpolated values. The temperature-dependent Cij values for GaxIn1xSb (x ¼ 0.78–0.95) were also measured using the pulse echo method between 4 and 300 K [3].

PROPERTIES OF SEMICONDUCTOR ALLOYS dC44 /dT dC12/dT dC11 /dT (107 dyn/cm2 K) (107 dyn/cm2 K) (107 dyn/cm2 K)

88

-6 -8 -10 -12 -14 -16 -4 -6 -8 -10 -12 0 -2 -4 -6 -8 0

(a)

ZnxCd1-xTe

(b)

(c)

0.2

0.4

0.6

x

0.8

1.0

Figure 3.9 dCij/dT versus x for ZnxCd1xTe at 300 K. The data represented by solid circles are taken from Queheillalt and Wadley [9] (x ¼ 0.04), while the open circles represent the endpoint binary data [1]

(b) Pressure effect

dC12 /dp

dC11 /dp

The pressure coefficient dCij/dp is a dimensionless quantity [1]. The linearly interpolated dCij/p values for GaxIn1xPyAs1y/InP are shown in Figure 3.10. The binary data are taken from Table 3.8 in Adachi [1]. Like dCij/dT in Figure 3.8, the dCij/dp versus y plots show very weak nonlinearity with respect to y. 6 5 4 3 2 6

Gax In1-x Py As1-y /InP

(a)

5 4

(b)

dC44 /dp

3 0.8 (c)

0.6 0.4 0.2 0

0.2

0.4

y

0.6

0.8

1.0

Figure 3.10 Linearly interpolated dCij/dp versus y for GaxIn1xPyAs1y/InP at 300 K. The binary dCij/dp values used in the calculation (Equation (A.6)) are taken from Adachi [1]

Maheswaranathan et al. [8] measured the pressure coefficients dCij/dp of CdTe and ZnxCd1xTe for p up to 4 kbar. They obtained dC11/dp ¼ 3.6 0.1, dC12/dp ¼ 4.4 0.1 (296 K) and dC44/dp ¼ 1.99 0.01 (196 K) for CdTe; dC11/dp ¼ 4.0 0.1, dC12/dp ¼ 4.4 0.1 (296 K) and dC44/dp ¼ 2.38 0.02 (196 K) for Zn0.48Cd0.52Te.

ELASTIC PROPERTIES

89

3.2 THIRD-ORDER ELASTIC CONSTANT No experimental data has been reported on the third-order elastic constants (Cijk) of group-IV, III–Vor II–VI semiconductor alloys. This necessitates the use of some sort of an interpolation scheme. The reported Cijk values for some non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Tables 3.11 and 3.12 of Adachi [1].

3.3 YOUNG’S MODULUS, POISSON’S RATIO AND SIMILAR PROPERTIES 3.3.1 Group-IV Semiconductor Alloy The general properties of various elastic moduli, such as Young’s modulus and Poisson’s ratio, are presented in Adachi [1]. The alloy Cij values can be estimated with good accuracy using the linear interpolation scheme (Section 3.1.2). Thus, the various elastic moduli can be calculated from the linearly interpolated Cij values. The expressions of the various elastic moduli can be found in Adachi [1]. As an example, the bulk moduli Bu calculated from the linearly interpolated Cij values of CxSi1x (dashed line) are illustrated in Figure 3.11. The endpoint and 3C-SiC data are shown by the open and solid circles, respectively [1]. These data show weak downward bowing (solid line). 500

Bu (GPa)

400

CxSi1-x

300 200 3C-SiC

100 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.11 Bulk modulus Bu versus x for CxSi1x at 300 K calculated using the linearly interpolated Cij values (dashed line). The endpoint and 3C-SiC values are shown by the open and solid circles, respectively [1]. These experimental data exhibit weak downward bowing (solid line)

Using a Monte Carlo simulation, Kelires [10] found that CxSi1x exhibits an accurate power-law dependence of Bu on the lattice constant a or, equivalently, on the average nearestneighbor distance d, over the whole composition range.

3.3.2 III–V Semiconductor Alloy A technique using XRD was demonstrated for the simultaneous determination of Poisson’s ratio P, lattice constant a and composition x for some III–V ternaries [11]. In Figure 3.12 P versus x has been plotted for (a) AlxIn1xAs, (b) GaxIn1xP and (c) GaxIn1xAs. The solid lines represent the results calculated from the linearly interpolated Cij values.

90

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.40 P

0.35 0.30

(a) Alx In1-x As

0.25 0.40 P

0.35 0.30

(b) Gax In1-xP

0.25 0.40 P

0.35 0.30 0.25

(c) Gax In1-x As

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.12 Poisson’s ratio P versus x for (a) AlxIn1xAs, (b) GaxIn1xP and (c) GaxIn1xAs at 300 K. The solid lines represent the P versus x curves calculated from the linearly interpolated Cij values. The solid circles show the experimental data taken from Hoke et al. [11], while the open circles represent the endpoint binary data taken from Adachi [1]

Figure 3.13 shows the bulk modulus Bu as a function of y for GaxIn1xPyAs1y/InP. The solid line represents the Bu versus y curve calculated from the linearly interpolated Cij values. The experimental data plotted are taken from Prins and Dunstan [12]. The experimental Bu data are found to be the same as InP to within 1%, while Ga0.47In0.53As (y ¼ 0) is 5% lower. 90 Gax In1-x Py As1-y /InP

Bu (GPa)

80 70 60 50

0

0.2

0.4

y

0.6

0.8

1.0

Figure 3.13 Bulk modulus Bu versus y for GaxIn1xPyAs1y/InP at 300 K. The solid line represents the Bu versus y curve calculated from the linearly interpolated Cij values. The solid circles represent the experimental data taken from Prins and Dunstan [12]. The open circle also represents the InP data taken from Adachi [1]

Caro et al. [13] determined Poisson’s ratio P of AlxGa1xAs using a HRXRD. They concluded that both the lattice parameter a and Poisson’s ratio P are in agreement with Vegard law.

3.3.3 II–VI Semiconductor Alloy The elastic constants Cij for the Be-based II–VI semiconductors, BeS, BeSe and BeTe listed in Table 3.1, are estimated from the simple Cij–a (lattice parameter) relationship in Adachi [1].

ELASTIC PROPERTIES

91

These elastic constants yield the bulk moduli Bu of 90, 81 and 67 GPa for BeS, BeSe and BeTe, respectively. On the other hand, the experimental data were Bu ¼ 92.2 1.8 GPa for BeSe and 66.8 0.7 GPa for BeTe if the pressure derivatives dBu/dp were fixed at 4 [14]. 80

10 c-ZnxCd1-xSe

8 6

Bu

40

4 dBu /dp

20 0

0

0.2

0.4

x

0.6

dBu /dp

Bu (GPa)

60

2 0.8

0 1.0

Figure 3.14 Bulk modulus Bu and pressure derivative dBu/dp versus x for c-ZnxCd1xSe at 300 K. The solid line represents the Bu versus y curve calculated using the linearly interpolated Cij values. The solid line for dBu/dp is also obtained from the linear interpolation scheme using the endpoint binary data in Adachi [1] (open triangles). The experimental data (x ¼ 0.9) are taken from Lin et al. [15]

The WDXS technique was employed to study the elastic properties of ZnxM1xSe (M ¼ Cd, Fe or Mn) [15]. Figure 3.14 shows the ZnxCd1xSe data for x ¼ 0.9. The Bu versus x curve is calculated from the linearly interpolated Cij values, while the dBu/dp curve is simply obtained from the linear interpolation between the endpoint values in Adachi [1]. The pressure derivative of Bu can now be written as [1] dBu 1 dC11 2 dC12 ¼ þ 3 dp 3 dp dp

ð3:2Þ

The bulk moduli Bu of ZnSexTe1x (0 x 1.0) have been determined using the WDXS [16]. These data are presented in Figure 3.15. The solid line shows the linear least-squares fit given by Bu ðxÞ ¼ 53:0 þ 13:5x

ð3:3Þ

80 ZnSexTe1-x

Bu (GPa)

70 60 50 40

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.15 Bulk modulus Bu versus x for ZnSexTe1x at 300 K. The experimental data are taken from Pellicer-Porres et al. [16]. The solid line represents the least-squares fit of Equation (3.3). The open circles show the endpoint binary data taken from Adachi [1]

92

PROPERTIES OF SEMICONDUCTOR ALLOYS

The x-dependent Young’s moduli Y have been determined for BexZn1xSe grown on GaP(100) and GaAs(100) by MBE [17]. The measured Y values increased almost linearly with increasing x. However, these data are slightly larger than the generally accepted values, e.g. about 10% larger for ZnSe.

3.4 MICROHARDNESS 3.4.1 Group-IV Semiconductor Alloy No detailed studies relating to the microhardness of group-IV semiconductor alloys have been found in the literature. The hardness values H for Si, diamond and 3C-SiC are shown graphically in Figure 3.16. The experimental data are taken from Table 3.23 in Adachi [1]. The 3C-SiC value deviates slightly from the weighted average of diamond and Si. 140 120

CxSi1-x

H (GPa)

100 3C-SiC

80 60 40 20 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.16 Microhardness H versus x for CxSi1x at 300 K. The endpoint and 3C-SiC values are plotted by the solid circles. These data are taken from Adachi [1]. The solid line represents the linear interpolation result between the endpoint elemental data

3.4.2 III–V Semiconductor Alloy Several authors have carried out measurements on the microhardness H of III–V semiconductor alloys. The H values for some (Al, Ga)- and (Ga, In)-based ternaries are shown in Figures 3.17 and 3.18, respectively. The experimental data in Figure 3.17 are taken from Caceres et al. [18] and Hjort et al. [19] and in Figure 3.18 from Bourhis and Patriarche [20] and Schenk and Silber [21]. The open circles represent the data taken from Adachi [1]. It can be seen from Figures 3.17 and 3.18 that the microhardness is almost linear with respect to x, except in the case of GaxIn1xP. The considerable strengthening observed in GaxIn1xP (x 0.5) was attributed to the high crystal friction as confirmed by the flow-stress values [20]. The microhardness anisotropy was determined for GaxIn1xPyAs1y/InP. Figure 3.19 shows the 3D representation of the Knoop hardness anisotropy on the (100) surfaces of GaxIn1xPyAs1y/InP with y as a parameter [22]. The ternary (y ¼ 0) and quaternary hardness anisotropy in Figure 3.19 share a general shape, which is fundamentally different from that of InP, having two or more maxima and one or more minima instead of one maximum and two minima. The major slip system in the diamond and zinc-blende structures is 1/2 {111}. Dislocations generated by plastic deformation, therefore, lie on the {111} planes with

ELASTIC PROPERTIES 24

93

12

21

10

H (GPa)

18 8

15 12

6

9

4

6 (a) w-AlxGa1-xN

3 0

0

0.2 0.4 0.6 0.8 1.0 x

2 0

(b) AlxGa1-xAs 0

0.2 0.4 0.6 0.8 1.0 x

Figure 3.17 Microhardness H versus x for (a) w-AlxGa1xN and (b) AlxGa1xAs at 300 K. The experimental data in (a) are taken from Caceres et al. [18] and in (b) from Hjort et al. [19]. The solid line in (b) shows the linear interpolation result between the endpoint binary data [1]

18

6 (a) GaxIn1-xP

H (GPa)

15 12

4

9

3

6

2

3

1

0

0

0.2 0.4 0.6 0.8 1.0 x

(b) GaxIn1-xSb

5

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 3.18 Microhardness H versus x for (a) GaxIn1xP and (b) GaxIn1xSb at 300 K. The experimental data in (a) are taken from Bourhis and Patriarche [20] and in (b) from Schenk and Silber [21] (heavy solid line). The solid lines show the linear interpolation results between the endpoint binary data [1]

1/2 Burgers vectors. The radically different shape of the anisotropy curves observed may suggest significant differences between the deformation behavior of the alloys and InP, which might be associated with different dislocation dynamics and even, perhaps, a primary slip system different from the , {111} system. The composition dependence of the average Knoop hardness H in Figure 3.19 shows that H increases with increasing y from the ternary value (5.2 GPa), peaking at y 0.5 (H 5.4 GPa), and decreasing with further increases of y (H 4 GPa at y ¼ 1.0) [22].

3.4.3 II–VI Semiconductor Alloy The microhardness of BeO has been reported to be H 0.92–13 GPa [23]. There has, however, been no experimental data for H in BeS, BeSe and BeTe. Alloying ZnSe with a more covalent II–VI compound such as BeSe may significantly alter the mechanical properties and eventually

94

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 3.19 Three-dimensional representation of microhardness anisotropy observed on (1 0 0)oriented GaxIn1xPyAs1y/InP with y as a parameter (y ¼ 0–1.0) at 300 K. [Reproduced with permission from D. Y. Watts and A. F. W. Willoughby, J. Mater. Sci. 23, 272 (1988), Copyright (1988) Springer]

lead to viable devices. In particular, both hardness and elastic modulus are expected to be enhanced by increasing the bond covalency. The composition dependence of H for BexZn1xSe has been investigated by several authors. We summarize these results in Figure 3.20. The experimental data are taken from Waag et al. [24] (open circles) and Paszkowicz et al. [25] (solid circles). The solid line also shows the experimental data of Grillo et al. [26]. Although there is a large difference in H, all these data show an increase in H with increasing x. The data of Grillo et al. [26] show a peak in H at x 0.7. 10 Bex Zn1-x Se

H (GPa)

8 6 4 2 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 3.20 Microhardness H versus x for BexZn1xSe at 300 K. The experimental data are taken from Waag et al. [24] (open circles) and Paszkowicz et al. [25] (solid circles). The solid line also represents the experimental data by Grillo et al. [26]

The microhardness H for ZnSexTe1x (0 x 0.06) and BexZn1xSeyTe1y (0 x 0.11) has been measured by Maruyama et al. [27]. These data show an increase in H with increasing Se or Be concentration. Figure 3.21 shows the experimental H data for ZnxHg1xSe as measured by Fang et al. [28]. The open circles represent the endpoint data taken from Adachi [1]. The solid line represents the linearly interpolated result. The experimental curve shows a pronounced peak at

ELASTIC PROPERTIES

95

Figure 3.21 Microhardness H versus x for ZnxHg1xSe at 300 K. [Reproduced with permission from S. Fang, L. J. Farthing, M.-F. S. Tang, and D. A. Stevenson, J. Vac. Sci. Technol. A 8, 1120 (1990). Copyright (1990), American Vacuum Society]. The solid line shows the linear interpolation result between the endpoint binary data [1]

x 0.7. Similarly, the experimental curve for ZnxCd1xTe obtained by Schenk and Dunog [29] showed a peak at x 0.7, as shown in Figure 3.22. A peak at x 0.7 was also observed in CdxHg1xTe [28]. The microhardness at x 0.7 in ZnxHg1xSe is about 1.6 GPa, which is at least twice the value of that in CdxHg1xTe. The microhardness H of CdxHg1xTe decreased with increasing temperature from 300 to 600 K, e.g. from H 0.7 GPa at 300 K to 0.2 GPa at 600 K for x ¼ 0.7 [30].

Figure 3.22 Microhardness H versus x for ZnxCd1xTe at 300 K. [Reproduced with permission from M. Schenk and L. T. H. Dunog, Semicond. Sci. Technol. 13, 335 (1998), Copyright (1998) Institute of Physics]. The solid line shows the linear interpolation result between the endpoint binary data [1]

Generally, isoelectronic doping in the order of ppm leads to a softening of the crystal lattice due to the vacancies in the lattice being filled with dopant atoms, and hence the etch-pit density is reduced, virtually without affecting the electrical properties of the material. Softening as a result of isoelectronic doping has been observed in In-doped GaAs [31] and in Zn-doped CdS [32].

96

PROPERTIES OF SEMICONDUCTOR ALLOYS

In conclusion of this section, the microhardness H of some tetrahedral semiconductor alloys shows a liner relationship between H and the alloy composition. More ionic semiconductor alloys, namely, II–VI alloys, however, show not only a clear upward bowing, but also a deviation from the parabolic behavior of the microhardness H. Such deviations lead to a peak in H at x 0.7 and not at x 0.5.

3.5 SOUND VELOCITY If the crystal density g and elastic stiffness Cij of a solid are known, the sound velocity v can be calculated from the simple relationship sﬃﬃﬃﬃﬃﬃ Cij v¼ g

ð3:4Þ

The detailed functional forms, in terms of Cij, of Equation (3.4) are shown in Tables 3.25 and 3.27 of Adachi [1]. The alloy Cij and g values can be approximated with good accuracy by the linear interpolation scheme. Thus, we can easily calculate the sound velocities propagating in the various crystallographic directions. For example, Figure 3.23 shows the calculated sound velocities propagating in the [110] direction in (a) AlxGa1xAs and (b) GaxIn1xPyAs1y/InP, where vLA corresponds to the longitudinal mode and vTA1 and vTA2 correspond to the slow and fast transverse modes, respectively. It can be seen that the sound velocities propagating in these alloys exhibit a weak nonlinear dependence on x or y.

7 6

7 6

vLA

v (105 cm/s)

5

(b) Gax In1-x PyAs1-y /InP vLA

5

4

4

vTA2

3

vTA2

3 vTA1

2 1 0 0

2 1

(a) AlxGa1-x As 0.2

0.4

0.6 x

vTA1

0.8

1.0

0 0

0.2

0.4

0.6

0.8

1.0

y

Figure 3.23 Sound velocities propagating in the [1 1 0] direction in (a) AlxGa1xAs and (b) GaxIn1x PyAs1y/InP, where vLA corresponds to the longitudinal mode and vTA1 and vTA2 correspond to the slow and fast transverse modes, respectively

ELASTIC PROPERTIES

97

Note that in piezoelectric semiconductors like GaAs and GaN, the sound velocity given by Equation (3.4) should be modified as sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Cij þ K 2 v¼ g

ð3:5Þ

where K2 is the electromechanical coupling constant [1], which leads to a piezoelectrically stiffened elastic constant if the sound wave is involved with piezoelectricity. The change in sound velocity due to piezoelectricity is only 0.1% for GaAs, but is 0.5% for GaN [33].

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] M. Mendik, M. Ospelt, H. von K€anel, and P. Wachter, Appl. Surf. Sci. 50, 303 (1991). [3] G. Galibert and G. Bougnot, Mater. Res. Bull. 9, 167 (1974). [4] G. Carlotti, D. Fioretto, L. Palmieri, G. Socino, A. Verdini, and C. Rigo, J. Phys.: Condens. Matter 8, 2265 (1996). [5] A. Hassine, J. Sapriel, P. L. Berre, P. Legay, F. Alexandre, and G. Post, J. Appl. Phys. 77, 6569 (1995). [6] F. C. Peiris, U. Bindley, J. K. Furdyna, H. Kim, A. K. Ramdas, and M. Grimsditch, Appl. Phys. Lett. 79, 473 (2001). [7] I. I. Andrusiv, G. M. Grigorovich, Y. V. Ilisavskiıˇ, M. A. Ruvinskiıˇ, and V. P. Shchetinin, Sov. Phys. Solid State 25, 139 (1983). [8] P. Maheswaranathan, R. J. Sladek, and U. Debska, Phys. Rev. B 31, 5212 (1985). [9] D. T. Queheillalt and H. N. G. Wadley, J. Appl. Phys. 83, 4124 (1998). [10] P. C. Kelires, Phys. Rev. B 55, 8784 (1997). [11] W. E. Hoke, T. D. Kennedy, and A. Torabi, Appl. Phys. Lett. 79, 4160 (2001). [12] A. D. Prins and D. J. Dunstan, Semicond. Sci. Technol. 4, 239 (1989). [13] L. D. Caro, C. Giannini, L. Tapfer, H.-P. Sch€onherr, L. D€aweritz, and K. H. Ploog, Solid State Commun. 108, 77 (1998). [14] H. Luo, K. Ghandehari, R. G. Greene, and A. L. Ruoff, Phys. Rev. B 52, 7058 (1995). [15] C.-M. Lin, D.-S. Chuu, J. Xu, E. Huang, W.-C. Chou, J.-Z. Hu, and J.-H. Pei, Phys. Rev. B 58, 16 (1998). [16] J. Pellicer-Porres, D. Martinez-Garcia, C. Ferrer-Roca, A. Segura, V. Mun˜oz-Sanjose, J. P. Itie, A. Polian, and P. Munsch, Phys. Rev. B 71, 035210 (2005). [17] S. E. Grillo, M. Ducarroir, M. Nadal, E. Tournie, and J.-P. Faurie, J. Phys. D: Appl. Phys. 35, 3015 (2002). [18] D. Caceres, I. Vergara, R. Gonzalez, E. Monroy, F. Calle, E. Mun˜oz, and F. Omnees, J. Appl. Phys. 86, 6773 (1999). [19] K. Hjort, F. Ericson, J.-A. Schweitz, C. Hallin, and E. Janzen, Thin Solid Films 250, 157 (1994). [20] E. L. Bourhis and G. Patriarche, Philos. Mag. Lett. 84, 373 (2004). [21] M. Schenk and C. Silber, J. Mater. Sci.: Mater. Electron. 9, 313 (1998). [22] D. Y. Watts and A. F. W. Willoughby, J. Mater. Sci. 23, 272 (1988). [23] L. Garrato and A. Rucci, Philos. Mag. 35, 1681 (1977). [24] A. Waag, F. Fischer, H.-J. Lugauer, T. Litz, T. Gerhard, J. N€ urnberger, U. Lunz, U. Zehnder, W. Ossau, G. Landwehr, B. Roos, and H. Richter, Mater. Sci. Eng. B 43, 65 (1997).

98

PROPERTIES OF SEMICONDUCTOR ALLOYS

[25] W. Paszkowicz, K. Godwod, J. Domagała, F. Firszt, J. Szatkowski, H. Me˛czy nska, S. Łe˛gowski, and M. Marczak, Solid State Commun. 107, 735 (1998). [26] S. E. Grillo, M. Ducarroir, M. Nadal, E. Tournie, and J.-P. Faurie, J. Phys. D: Appl. Phys. 35, 3015 (2002). [27] K. Maruyama, K. Suto, and J. Nishizawa, Jpn. J. Appl. Phys. 39, 5180 (2000). [28] S. Fang, L. J. Farthing, M.-F. S. Tang, and D. A. Stevenson, J. Vac. Sci. Technol. A 8, 1120 (1990). [29] M. Schenk and L. T. H. Dunog, Semicond. Sci. Technol. 13, 335 (1998). [30] J. F. Barbot, G. Rivaud, H. Garem, C. Blanchard, J. C. Desoyer, D. Le-Scoul, J. L. Dessus, and A. Durand, J. Mater. Sci. 25, 1877 (1990). [31] S. Kouba€ıti, C. Levade, J. J. Couderc, and G. Vanderschaeve, Eur. Phys. J. Appl. Phys. 1, 141 (1998). [32] K. Balakrishnan, J. Kumar, and P. Ramasamy, J. Mater. Sci. Lett. 14, 720 (1995). [33] C. Deger, E. Born, H. Angerer, O. Ambacher, M. Stutzmann, J. Hornsteiner, E. Riha, and G. Fischerauer, Appl. Phys. Lett. 72, 2400 (1998).

4 Lattice Dynamic Properties 4.1 PHONON DISPERSION RELATIONSHIPS Theoretical work on the lattice dynamics of semiconductor alloys has been carried out by several authors. For example, Myles [1] evaluated the spectral density of phonon states for 1D mass-disordered alloys using a generalized embedded-cluster method. Baroni et al. [2] studied the lattice vibronic properties of AlxGa1xAs using large supercells to simulate the disorder and ab initio interatomic force constants. They found that there are well-defined AlAs- and GaAslike phonon dispersions for any concentration, in agreement with experimental evidence [3]. In addition to broadening phonon states with definite wavevectors, alloying also narrows the optical phonon branches and lowers the longitudinal modes more than the transverse modes, thus reducing the LO–TO splitting. The acoustic phonon bands are in contrast also found to be rather insensitive to the alloy composition.

4.2 PHONON FREQUENCY 4.2.1 General Considerations Lattice vibronic properties in semiconductor alloys have received a great deal of attention over a long period of time [4]. The defect-induced local or gap modes for small concentrations of impurities are broadened into vibrational bands for high impurity concentrations as in solid solutions. In an AxB1xC alloy, such vibrational bands exhibit either one-mode or twomode behavior (or more rigorously, three different types of mode behavior, namely, one-, two- and one-two-mode (mixed-mode) behaviors; see Figure 4.1). In a one-mode system (Figure 4.1(a)), such as most I–VII alloys, a single set of long-wavelength optical phonons appear. The one-mode phonon spectrum is approximately constant in strength but varies in energy as the alloy composition is varied from one end member to another. The two-mode system (Figure 4.1(b)), which is common for III–V ternaries, exhibits two distinct sets of optical modes with frequencies characteristic of each end member and strengths roughly proportional to the respective concentration. The one-two-mode system exhibits a single mode over only a part of the composition range, with two modes observed over the remaining range of composition (Figures 4.1(c) and 4.1(d)). A number of models have been proposed to explain the so-called multi-mode behavior in solid solutions [5]. Of these different models, the MREI model of Chang and Mitra [5,6] appears to be the most successful. In the MREI model, if an alloy AxB1xC has the relationship MA < mBC Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

ð4:1Þ Sadao Adachi

100

PROPERTIES OF SEMICONDUCTOR ALLOYS

LO 1

LO 1

LO 1

LO

ω LO, TO

TO 1

TO 1

LO 2

TO 1 LO 2

LO 2

TO TO 2

TO2

TO 2

Local mode Gap mode

(a) 0

0.5 x

1.0 0

(b) 0.5 x

1.0 0

(c) 0.5 x

1.0 0

(d) 0.5 x

1.0

Figure 4.1 Four different types of long-wavelength phonon mode behavior in ternary alloy: (a) onemode; (b) two-mode; (c) one-two-mode (1); (d) one-two-mode (2) 1 1 it exhibits two-mode behavior. Here,m1 BC ¼ MB þ MC is the reduced mass of the binary material BC. The opposite is true for one-mode behavior. In other words, for an alloy to exhibit two-mode (one-mode) behavior it must (must not) have one substituting element whose mass is smaller than the reduced mass of the compound formed by the other two elements. Given the masses of the end members, the MREI model can predict whether an alloy will show one- or two-mode behavior and also the dependence of the optical phonon frequencies on x [5, 6]. Table 4.1 summarizes the long-wavelength optical phonon frequencies, h¯ vLO and h¯ vTO, for a number of cubic group-IV, III–Vand II–VI semiconductors at 300 K and Table 4.2 lists those for some hexagonal III–V and II–VI semiconductors at 300 K. In an ordered alloy Ga0.5In0.5P, four additional phonon modes at 60, 205, 310 and 354 cm1, attributed to spontaneous ordering in this material, have been identified and explained using various experimental techniques [7]. However, a major obstacle to further enhancing the understanding of this subject is the lack of a theoretical model that can satisfactorily explain the experimental optical phonon frequencies and selection rules in ordered alloys. In the following, the data mainly refers to fully disordered semiconductor alloys.

4.2.2 Room-temperature Value (a) Group-IV semiconductor alloy The experimental long-wavelength optical phonon frequencies vLO and vTO for 3C-SiC, together with those for diamond and Si, are shown in Figure 4.2. 3 C-SiC is considered to be an ordered alloy, or more succinctly, it is a compound, not an alloy. Note that for diamond-type structures the LO and TO branches are degenerate at q ¼ 0 and thus vLO ¼ vTO. The solid line in Figure 4.2 shows the linear interpolation result between Si (x ¼ 0) and diamond (x ¼ 1.0). The 3C-SiC values can be satisfactorily interpreted by the average values of Si and diamond. SixGe1x has three types of cell and consequently shows multi-mode behavior consisting of three main peaks due to the vibrations of SiSi, GeGe and SiGe pairs (Table 4.3). The composition dependence of the SiSi, SiGe and GeGe mode frequencies for SixGe1x

LATTICE DYNAMIC PROPERTIES

101

Table 4.1 Long-wavelength optical phonon frequencies, h¯ vLO and h¯ vTO, for some cubic group-IV, IIIV and IIVI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt h¯ vLO (cm1)

h¯ vTO (cm1)

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

1332 519.2 301 200 972

1332 519.2 301 200 796

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

1305 828.9 902 501.0 402 340.0 739 402.5 292 233 586 346.4 241.4 190.7

1054.7 799 655 439.4 362 318.7 553 365.3 268 224 455 304.5 219.6 179.7

II–VI

BeSe (zb) BeTe (zb) MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

576 502 725 425 340 292 350.5 252 210 478 303a 211a 167 224 174 135

496 461 401 327 237 235 272.0 205 181 262 237a 169a 139 177 132 116

System

Material

IV

a

Calculated or estimated

is shown in Figure 4.3(a). The experimental data were obtained from Pezzoli et al. [8]. The homopolar-bond frequencies vary almost linearly with x, while the heteropolar-bond frequency shows a maximum at x 0.5. These can be written as (in cm1) vSiSi ðxÞ ¼ 52167x

ð4:2aÞ

102

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 4.2 Long-wavelength optical phonon frequencies for some hexagonal III–V and II–VI semiconductors at 300 K. h ¼ hexagonal (P63/mmc (D6h)); w ¼ wurtzite System

Phonon frequency (cm1)

Material E2 low

A1 (TO)

E1 (TO)

E2 high

A1 (LO)

E1 (LO)

III–V

BN (h) AlN (w) GaN (w) InN (w)

49 248 144 87

770 610 533 457

1383 670 560 490

1367 657 569 475

778 890 736 588

1610 915 743 582

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

340 100 65 41 34

680 380 270 233 166

724 410 273 239 170

684 439 281 255

1083 576 350 301 210

1098 587 350 304 211

Cx Si1-x

3C-SiC

ω LO, TO (cm-1)

1500 1200

ω LO

900

ω TO

600 300

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.2 Long-wavelength optical phonon frequencies vLO and vTO for 3C-SiC at 300 K, together with those for diamond and Si. The solid line represents the linear interpolation result between the endpoint elemental data

Table 4.3 Long-wavelength optical phonon mode observed in some group-IV semiconductor alloys Alloy

Phonon mode

Reference

SiGe CSiGe SiGeSn

SiSi, GeGe, SiGe SiSi, GeGe, CSi, CGe (?), SiGe SiSi, GeGe, SiGe, SnSn

a b c

F. Pezzoli et al., Mater. Sci. Eng. B 124–125, 127 (2005) C 0.3 at% (M. Melendez-Lira et al., Phys. Rev. B 54, 12866 (1996)) c Si 20 at%, Sn 10 at% (V. R. DCosta et al., Phys. Rev. B 76, 035211 (2007)) a b

LATTICE DYNAMIC PROPERTIES

103

Figure 4.3 (a) Three main optical phonon frequencies due to the vibrations of SiSi, SiGe and GeGe pairs versus x for SixGe1x at 300 K. (b) Relative Raman intensities against x for SixGe1x at 300 K. [Reprinted with permission from Mater. Sci. Eng. B, Raman spectroscopy of Si1xGex epilayers by F. Pezzoli et al., 124–125, 127. Copyright (2005), Elsevier]

vGeGe ðxÞ ¼ 280 þ 19x

ð4:2bÞ

for the homopolar-bond modes and vSiGe ðxÞ ¼ 400 þ 24:5x4:5x2 33:5x3

ð4:3Þ

for the heteropolar-bond mode. The corresponding Raman intensities are plotted in Figure 4.3(b). The probability of finding SiSi, SiGe and GeGe vibrating pairs is proportional to the relative numbers of the bond types: x2, 2x(1 x) and (1 x)2, respectively. The experimental data in Figure 4.3(b) follow this statistic very well. The ordering effect and/or compositional fluctuation should influence the vibronic properties of alloys, and in particular, the relative intensities and linewidths of the Raman modes. Tsang et al. [9] measured the Raman spectra of compositionally ordered Si0.5Ge0.5 layers and compared them to the spectrum of a random alloy. They observed changes in the relative intensities of the different optical phonons, suggesting that the ordering is associated with an increase in the number of homopolar bonds and a decrease in the number of heteropolar bonds. The Raman scattering data also suggested that the ordering is not complete; the changes in the Raman intensities are quantitatively consistent with XRD-estimated ordering of 80%. The effects of substitutional carbon in SixGe1x have been studied by several authors [10–12]. Because of the significant difference in covalent bond radii between Si and C atoms, the C defect in the Si lattice is surrounded by a considerable strain field, with substitutional defect bonds under tensile strain and interstitial bonds under compressive strain. A substitutional C defect in SixGe1x is expected to be surrounded by an even stronger strain field than

104

PROPERTIES OF SEMICONDUCTOR ALLOYS

that in pure Si, due to the increase in the C bond lengths with the Ge atoms. Interstitial C defects will be under smaller compressive strain due to the increase in the average lattice constant with Ge. The experimental frequencies of the SiSi, GeGe and SiGe modes in SixGe1x increased as a function of C concentration, which can be explained qualitatively in terms of the large bond distortions caused by the lattice mismatch between SixGe1x and diamond [10]. A number of phonon modes associated with the substitutional C defects in SixGe1x have been detected and attributed to localized phonon modes of C defects with different nearest-neighbor configurations of Si and Ge atoms (Table 4.3). (b) III–V semiconductor alloy Most IIIV ternaries exhibit two-mode behavior. Some IIIV ternaries exhibit one- or onetwo-mode behavior. These are summarized in Table 4.4. The long-wavelength optical phonon Table 4.4 Behavior of the long-wavelength optical phonon modes in some III–V semiconductor alloys. zb ¼ zinc-blende; w ¼ wurtzite; O ¼ one mode; T ¼ two mode; O-T ¼one-two mode; Tr-F ¼ three-four mode; Tr ¼ three mode; F ¼ four mode; T-Tr ¼ two-three mode Alloy

Material

Behavior

Reference

Ternary

AlGaN (zb) AlGaN (w) AlInN (w) AlGaP (zb) AlGaAs (zb) AlGaSb (zb) AlInP (zb) AlInAs (zb) AlInSb (zb) GaInN (zb) GaInN (w) GaInP (zb) GaInAs (zb) GaInSb (zb) AlAsSb (zb) GaNP (zb) GaNAs (zb) GaPAs (zb) GaPSb (zb) GaAsSb (zb) InPAs (zb) InPSb (zb) InAsSb (zb)

O (LO), T (TO) T (E1(TO)), O (others) O (A1(LO), E1(LO)), T (others) O O (E1(TO)) T T T T T T O O T T O-T O T T T T T T T O-T

a b c d e f g h i j k l m n o p q r s t u v w x y

AlGaPAs (zb) AlGaAsSb (zb) GaInPSb (zb)

Tr-F Tr F

z aa ab

Quaternary

(continued)

LATTICE DYNAMIC PROPERTIES

105

Table 4.4 (Continued) Alloy

Material

Behavior

Reference

GaInPAs/InP (zb) GaInPAs/GaAs (zb) GaInAsSb (zb) AlGaInP/GaAs (zb) AlGaInAs/InP (zb) InPAsSb (zb)

F F Tr T-Tr Tr Tr

ac ad ae af ag ah

H. Harima et al., Appl. Phys. Lett. 74, 191 (1999) M. Kazan et al., J. Appl. Phys., 100, 013508 (2006) c V. Y. Davydov et al., Phys. Rev. B 65, 125203 (2002) d M. S. Liu et al., J. Appl. Phys. 90, 1761 (2001) e A. Kasic et al., Appl Phy. Lett. 78, 1526 (2001) f G. Armelles et al., Solid State Commun. 65, 779 (1988) g D. J. Lockwood and Z. R. Wasilewski, Phys. Rev. B 70, 155202 (2004) h R. Ferrini et al., Phys. Rev. B 56, 7549 (1997) i H. Asahi et al., J. Appl. Phys. 65, 5007 (1989) j S. Emura et al., J. Appl. Phys. 62, 4632 (1987) k V. P. Gnezdilov et al., J. Appl. Phys. 74, 6883 (1993) l K. Torii et al., Appl. Phys. Lett. 82, 52 (2003) m S. Hernandez et al., J. Appl. Phys. 98, 013511 (2005) n B. Jusserand and S. Slempkes, Solid State Commun. 49, 95 (1984) o Z. S. Piao et al., Phys. Rev. B 50, 18644 (1994) p Z. C. Feng et al., Can. J. Phys. 69, 386 (1991) q H. C. Lin et al., Solid State Commun. 107, 547 (1998) r G. Leibiger et al., Appl. Phys. Lett. 79, 3407 (2001) s T. Prokofyeva et al., Appl. Phys. Lett. 73, 1409 (1998) t G. Armelles et al., Appl. Phys. Lett. 68, 1805 (1996) u Y. T. Cherng et al., J. Appl. Phys. 65, 3285 (1989) v T. C.McGlinn et al., Phys. Rev. B 33, 8396 (1986) w D. J. Lockwood et al., J. Appl. Phys. 102, 033512 (2007) x M. J. Jou et al., J. Appl. Phys. 64, 1472 (1988) y N. L. Rowell et al., J. Vac. Sci. Technol. A 22, 935 (2004) z P. N. Sen and G. Lucovsky, Phys. Rev. B 12, 2998 (1975) aa D. H. Jaw et al., J. Appl. Phys. 69, 2552 (1991) ab D. H. Jaw and G. B. Stringfellow, J. Appl. Phys. 72, 4265 (1992) ac T. Sugiura et al., Jpn. J. Appl. Phys. 37, 544 (1998) ad T. Sugiura et al., Jpn. J. Appl. Phys. 32, 2718 (1993) ae D. H. Jaw et al., J. Appl. Phys. 66, 1965 (1989) af T. Hofmann et al., Phys. Rev. B 64, 155206 (2001) ag R. Manor et al., Phys. Rev. B 56, 3567 (1997) ah L.-C. Chen et al., Jpn. J. Appl. Phys. 37, L1365 (1998) a b

frequencies vLO and vTO versus x for (a) c-AlxGa1xN and (b) c-GaxIn1xN are shown in Figure 4.4. The experimental data for c-AlxGa1xN are taken from Harima et al. [13] and for c-GaxIn1xN from Tabata et al. [14] and Torii et al. [15]. The LO phonon frequencies in Figure 4.4(a) exhibit one-mode behavior, while the twomode behavior is observed for the TO phonon frequencies. The mass criterion of Equation (4.1) suggests that AlxGa1xN may exhibit one-mode behavior (MAl,Ga > mAlN,GaN). Harima

106

PROPERTIES OF SEMICONDUCTOR ALLOYS 1000

800

(a)

ω LO, TO (cm-1)

900

(b) c-Gax In1-x N

c-AlxGa1-x N

800

700 LO

LO

600 700 TO TO (AlN)

600

500

TO (GaN)

500

0

0.2

0.4

0.6

0.8

1.0

400

0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 4.4 Long-wavelength optical phonon frequencies vLO and vTO versus x for (a) c-AlxGa1xN and (b) c-GaxIn1xN at 300 K. The experimental data for c-AlxGa1xN are taken from Harima et al. [13] and for c-GaxIn1xN from Tabata et al. [14] and Torii et al. [15]. The solid line in (a) shows the linear interpolation result between the endpoint binary data (LO). The solid lines in (b) represent the linear interpolation results of Equation (4.4)

et al. [13] calculated the phonon frequencies using the MREI model and considered that the two-mode behavior of vTO is a consequence of the different vibrating masses. In Figure 4.4(b), clear one-mode phonon behavior of c-GaxIn1xN can be seen, in agreement with the criterion of Equation (4.1) (MGa,In > mGaN,InN). The solid lines represent the linear interpolation results (in cm1) vLO ðxÞ ¼ 739153x

ð4:4aÞ

vTO ðxÞ ¼ 55398x

ð4:4bÞ

Figure 4.5 shows the LO and TO phonon frequencies as a function of x for AlxGa1xAs. The experimental data are taken from Jusserand [16]. Only the AlAs-like LO mode exhibits weak nonlinearity with respect to x. Each phonon frequency can be expressed as (in cm1) vLO;AlAs ðxÞ ¼ 354 þ 81x33x2

ð4:5aÞ

vTO;AlAs ðxÞ ¼ 354 þ 8x

ð4:5bÞ

vLO;GaAs ðxÞ ¼ 29237x

ð4:6aÞ

vTO;GaAs ðxÞ ¼ 26813x

ð4:6bÞ

The two-mode behavior in AlxGa1xAs is the most prominent disorder-induced effect (MAl < mGaAs). Additional disorder-induced effects in AlxGa1xAs have been observed, i.e. an asymmetric line broadening and an activation of new phonon bands [16]. A low energy GaAslike LO tail developed when the concentration of Al increased, and vice versa. When this concentration becomes very large, an additional line appears on the lower energy side. Apart from this broadening, additional phonon bands are observed in the TA (100 cm1) and LA

LATTICE DYNAMIC PROPERTIES

107

400

ω LO, TO (cm-1)

LO (AlAs)

350

TO (AlAs)

AlxGa1-xAs 300 LO (GaAs)

250

TO (GaAs)

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.5 Long-wavelength optical phonon frequencies vLO and vTO versus x for AlxGa1xAs at 300 K. The open squares represent the endpoint binary data. The solid lines show the results calculated using Equations (4.5) and (4.6)

range (200 cm1). The asymmetric broadening and the emergence of additional phonon bands can be explained by a disorder activated relaxation of the q ¼ 0 wavevector selection rule. The LO and TO phonon frequencies for GaxIn1xSb determined by Raman scattering at 80 K by Feng et al. [17] are shown in Figure 4.6. They also reported the room-temperature data, which are essentially the same as those at 80 K. In Figure 4.6, the so-called one-two-mode behavior is observed; however, the mass criterion of Equation (4.1) indicates that the alloy will exhibit one-mode behavior (MGa,In > mGaSb,InSb). The one-two-mode behavior was also confirmed using IR spectroscopy [18].

ω LO, TO (cm-1)

250 LO (GaSb)

225

TO (GaSb) 200

LO (InSb) TO (InSb)

175

Gax In1-x Sb

T= 80 K 150

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.6 Long-wavelength optical phonon frequencies vLO and vTO versus x for GaxIn1xSb at 80 K. [Reproduced with permission from Z. C. Feng, S. Perkowitz, R. Rousina, and J. B. Webb, Can. J. Phys. 69, 386–389 (1991), Copyright (1991) NRC Research Press]

108

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.7 Long-wavelength optical phonon frequencies vLO and vTO versus y for GaxIn1xPyAs1y/ InP at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Raman scattering study of InGaAsP quaternary alloys grown on InP in the immiscible region by T. Sugiura et al., 37, 544. Copyright (1998) Japanese Society of Pure and Applied Physics] The open circles represent the InP data

The long-wavelength optical phonon behaviors in GaxIn1xPyAs1y/InP have been studied by Raman and IR spectroscopy [19]. In Figure 4.7 the vLO and vTO frequencies versus y for GaxIn1xPyAs1y/InP are illustrated graphically. The experimental data are taken from Sugiura et al. [20]. The data fall into four separate bands, that is, a four-mode category, except for the GaAs mode at y > 0.6. The composition dependence of vLO and vTO for (AlxGa1x)0.48In0.52As/InP is shown in Figure 4.8. The experimental data were obtained by Raman scattering [21]. Three modes, AlAs-, GaAs- and InAs-like modes, dominate the Raman spectra in (AlxGa1x)0.48In0.52As/ InP. The GaAs- and InAs-like modes vary almost linearly with x. The AlAs-like TO mode also varies linearly with x, but its LO branch exhibits weak nonlinearity with respect to x. The one-mode behavior of AlAsxSb1x and two-mode behavior of GaPxAs1x, GaPxSb1x and InPxAs1x in Table 4.4 agree with the mass criterion of Equation (4.1); however, the twomode behavior observed in GaxIn1xP and GaAsxSb1x is contrary to this criterion. Let us consider GaPxAs1x and GaxIn1xP, the former shows two-mode behavior, while the latter shows one-mode (or a very weak two-mode) behavior. These behaviors are easily understood by noting that the optical-phonon DOS of GaP and GaAs do not overlap unlike those of GaP and InP which do overlap (but in a narrow frequency range). Thus, the two-mode behavior of GaPxAs1x is expected from Equation (4.1) (MP < mGaAs). Because MGa > mGaP,InP, the MREI model predicts one-mode behavior in GaxIn1xP.

LATTICE DYNAMIC PROPERTIES

109

Figure 4.8 Long-wavelength optical phonon frequencies vLO and vTO versus x for (AlxGa1x)0.48 In0.52As/InP at 300 K. [Reproduced with permission from R. Manor, O. Brafman, and R. F. Kopf, Phys. Rev. B 56, 3567–3570 (1997). Copyright (1997) American Physical Society]

(c) II–VI semiconductor alloy II–VI ternaries grow either in the zinc-blende or wurtzite structure and mostly exhibit one- or two-mode behavior, as summarized in Table 4.5. Some II–VI ternaries exhibit a variation with composition that is intermediate between one- and two-mode. Figure 4.9 shows the long-wavelength optical phonon frequencies vLO and vTO as a function of x for ZnxCd1xS. The experimental data are taken from Lucovsky et al. [22]. Since ZnxCd1xS crystallizes in the wurtzite structure, the experimental data produced by Lucovsky et al. shows a small anisotropy splitting (6 cm1) between A1 (LO, TO) and E1 (LO, TO) modes for all values of x. For clarity, however, the averaged vLO and vTO values have been plotted in Figure 4.9. ZnxCd1xS serves a typical example of the one-mode phonon behavior. Figure 4.10 shows the LO and TO phonon frequencies for CdxHg1xTe measured by IR spectroscopy at 77 K [23]. Like ZnxHg1xTe [24], CdxHg1xTe exhibits two-mode behavior. However, the ZnTe-like TO frequency in ZnxHg1xTe increased with increasing Zn content, while the CdTe-like TO phonon mode in CdxHg1xTe (Figure 4.10) decreased with increasing Cd content. This could be due to the fact that the ZnxHg1xTe lattice constant decreases with increasing Zn content but the CdxHg1xTe lattice constant increases with increasing Cd content. Note that the MREI model predicts ZnxHg1xTe to be of the two-mode type (MZn < mHgTe) and CdxHg1xTe to be of the one-mode type (MCd,Hg > mCdTe,HgTe). Both ZnxCd1xSe and ZnSexTe1x exhibit an intermediate-mode behavior [25,26]. As an example, the data for ZnSexTe1x is shown in Figure 4.11 [25]. Not only are the one-mode LO and TO phonons (LO1 and TO1) but also a new LO2–TO2 pair inside the reststrahlen band.

110

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 4.5 Behavior of the long-wavelength optical phonon modes in some II–VI semiconductor alloys. zb ¼ zinc-blende; w ¼ wurtzite; O ¼ one mode; T ¼ two mode; I ¼ intermediate mode; Tr ¼ three mode Alloy

Material

Behavior

Reference

Ternary

BeZnSe BeZnTe MgZnO (zb) MgZnO (w) MgZnO (w) MgZnS MgZnSe MgZnTe MgCdTe ZnCdS ZnCdSe ZnCdTe ZnHgTe CdHgTe ZnSSe ZnSTe ZnSeTe CdSSe CdSTe CdSeTe

Tr Tr T O T (E1), O (A1) O T T T O I T T T T T I T T T

a b c d e f g h i j k l m n o p q o r s

Quaternary

MgZnSSe MgZnSeTe MgZnCdTe ZnCdHgTe CdSSeTe

Tr T Tr Tr Tr

f t h u v

Showing extra BeSe-like mode (O. Pages et al., Phys. Rev. B 70, 155319 (2004)) Showing extra BeTe-like mode (O. Pages et al., Appl. Phys. Lett. 80, 3081 (2002)) c J. Chen and W. Z. Shen, Appl. Phys. Lett. 83, 2154 (2003) d 0 x < 0.3 (Z. P. Wei et al., Phys. Status Solidi C 3, 1168 (2006)) e x0.47–0.60 (J.Chen and W. Z. Shen, Appl. Phys. Lett. 83, 2154 (2003)) f D. Wang et al., J. Appl. Phys. 80, 1248 (1996) g D. Huang et al., Appl. Phys. Lett. 67, 3611 (1995) h R. Vogelgesang et al., J. Raman Spectrosc. 27, 239 (1996) i E. Oh et al., Phys. Rev. B 48, 15040 (1993) j M. Ichimura et al., Phys. Rev. B 46, 4273 (1992) k R. G. Alonso et al., Phys. Rev. B 40, 3720 (1989) l D. N. Talwar et al., Phys. Rev. B 48, 17064 (1993) m M. P. Volz et al., Solid State Commun. 75, 943 (1990) n S. P. Kozyrev et al., Sov. Phys. Solid State 34, 1984 (1992) o I. F. Chang and S. S. Mitra, Phys. Rev. 172, 924 (1968) p Y.-M. Yu et al., J. Appl. Phys. 95, 4894 (2004) q T. R. Yang and C. C. Lu, Physica B 284–288, 1187 (2000) r R. Pal et al., J. Phys. D: Appl. Phys. 26, 704 (1993) s Z. C. Feng et al., J. Cryst. Growth 138, 239 (1994) t H. Makino et al., J. cryst. Growth 214/215, 359 (2000) u J. Polit et al., Phys. Status Solidi B 208, 21 (1998) v V. M. Burlakov et al., Phys. Status Solidi B 128, 389 (1985) a b

LATTICE DYNAMIC PROPERTIES

111

ω LO, TO (cm-1)

400 ZnxCd1-xS

350

ω LO

300 ω TO

250 200

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.9 Long-wavelength optical phonon frequencies vLO and vTO versus x for ZnxCd1xS at 300 K. The experimental data are taken from Lucovsky et al. [22]. The solid lines show the linearly interpolated results between the endpoint binary data

Figure 4.10 Long-wavelength optical phonon frequencies vLO and vTO versus x for CdxHg1xTe at 77 K. [Reprinted with permission from J. Baars and F. Sorger, Solid State Commun. 10, 875 (1972), Copyright (1972) Elsevier]

Pages et al. [27, 28] investigated the Raman spectra of BexZn1xSe and BexZn1xTe. The TO modes were of particular interest because they consist of quasi-independent oscillators and thereby carry clear information. In the LO symmetry, complexity arose due to coupling via the macroscopic polarization field. They observed the atypical TO one-bond ! two-mode behavior in the vibrational range of the stiff Be–VI bond in BexZn1xSe and BexZn1xTe. This was explained by using a double-branch percolation picture which discriminates between vibrations within the randomly formed hard Be-rich host region and the soft Zn-rich region. The resulting phonon frequency versus composition plots showed that the (Be, Zn)–VI ternaries exhibit a three-mode (two usual modes plus one mode) behavior [27, 28] . The composition dependence of vLO and vTO for MgxZn1xSySe1y/GaAs is shown in Figure 4.12. The experimental data were obtained by Raman scattering [29]. In brief, we can expect four-mode behavior (AB-, AC-, BC- and BD-like) in an AxB1xCyD1y alloy. However, the data in Figure 4.12 reveal three-mode behavior (MgSe-, ZnSe- and MgZnS-like). Similarly,

112

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.11 Long-wavelength optical phonon frequencies vLO and vTO versus x for ZnSexTe1x at 300 K. [Reprinted with permission from Physica B, Infrared studies and optical characterization of ZnSe1xTex molecular beam epitaxial films by T. R. Yang and C. C. Lu, 284–288, 1187. Copyright (2000), Elsevier] The open circles represent the InP data 400 LO (MgZnS)

ω LO, TO (cm-1)

350 LO (MgSe)

300 LO

250 ZnSe-like 200

TO

Mgx Zn1-x S y Se1-y /GaAs

150

0

0.2

0.4

0.6

0.8

1.0

y

Figure 4.12 Long-wavelength optical phonon frequencies vLO and vTO versus y (S) for MgxZn1xSySe1y/GaAs at 300 K. [Reprinted with permission from D. Wang et al., J. Appl. Phys. 80, 1248 (1996). Copyright (1996), American Institute of Physics]

MgxZn1xSeyTe1y showed two-mode behavior (MgSeTe- and ZnSeTe-like), not four-mode behavior [30]. As expected, both ZnxCd1xHg1xyTe and CdSxSe1xTe1xy exhibited threemode behavior (Table 4.5).

4.2.3 External Perturbation Effect (a) Group-IV semiconductor alloy The phonon frequency is dependent both on temperature T and pressure p. The longwavelength optical phonon frequency vop versus T can be expressed as [31] vop ðTÞ ¼ vop ð0Þ

aT 2 T þb

ð4:7Þ

LATTICE DYNAMIC PROPERTIES

113

Figure 4.13 Hydrostatic-pressure dependence of the optical phonon frequency vop for Si0.55Ge0.45 at 300 K. The experimental data are taken from Sui et al. [32]. The bulk Si and Ge data are taken from Adachi [33]

where vop(0) is the T ¼ 0 K value, a is in cm1 per degree Kelvin and b is a quantity proportional to the Debye temperature (in Kelvins). No detailed data on the temperature dependence of vop ¼ vLO,TO in group-IV semiconductor alloys has been reported. The pressure dependence of vop in Si0.55Ge0.45 determined by Raman scattering is shown in Figure 4.13. The experimental data are taken from Sui et al. [32]. The pressure coefficients dv/ dp obtained from these plots are 7, 5 and 4 cm1/GPa for the SiSi, SiGe and GeGe modes, respectively. The solid lines in Figure 4.13 show the bulk Si and Ge data [33]. (b) III–V semiconductor alloy Figure 4.14 (a) shows the vLO versus T plots for the GaAs-like mode in AlxGa1xAs. The experimental data are taken from Jimenez et al. [34]. The temperature variations are almost linear in the range between 300 and 650 K. The corresponding coefficient dvLO/dT for AlxGa1xAs is plotted in Figure 4.14 (b) [34]. The GaAs (x ¼ 0) and AlAs (x ¼ 1.0) data are also shown by the solid and open triangles, respectively [35]. It can be seen that the temperature coefficients are almost composition independent (dvLO/dT2 102 cm1/K). The pressure dependence of the LO phonon frequencies in Al0.58Ga0.42As is shown in Figure 4.15. The LO phonon frequencies were measured by Raman scattering up to 7 GPa [36]. The pressure coefficients for the LO and TO modes in AlAs and GaAs were reported to be 5 (AlAs) and 4 cm1/GPa (GaAs), respectively [36]. The slopes for the experimental Al0.58Ga0.42As data in Figure 4.15 are nearly the same as those for AlAs and GaAs. The pressure coefficients dvLO,TO/dp for the AlAs- and GaAs-like LO and TO modes for AlxGa1xAs are plotted as a function of x in Figure 4.16. The experimental data are taken from Holtz et al. [36]. Although the experimental data largely scatter, we can see that they fall in the range 5.3 1.3 cm1/GPa, as shown by the vertical bar.

114

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.14 (a) Temperature dependence of the GaAs-like LO phonon frequency vLO for AlxGa1xAs. The data for bulk GaAs are also shown. [From J. Jimenez, E. Martın, A. Torres, and J. P. Landesman, Phys. Rev. B 58, 10463–10469 (1998). Copyright (1998) American Physical Society.] (b) Temperature coefficient dvLO/dT versus x for AlxGa1xAs at 300 K. The experimental data are taken from Jimenez et al. [34]. The solid and open triangles represent the endpoint binary data taken from Adachi [35]

Figure 4.15 Hydrostatic-pressure dependence of the AlAs- and GaAs-like LO phonon frequencies for Al0.58Ga0.42As at 300 K. The experimental data are taken from Holtz et al. [36]. The bulk GaAs data are also taken from Adachi [35]

LATTICE DYNAMIC PROPERTIES

115

dω LO,TO /dp (cm-1/GPa)

8 7 6 5 4 3 2

LO (AlAs) TO (AlAs) LO (GaAs) TO (GaAs)

AlxGa1-x As

1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.16 Pressure coefficients dvLO,TO/dT for the AlAs- and GaAs-like LO and TO modes in AlxGa1xAs at 300 K. The experimental data are taken from Holtz et al. [36]. The vertical bar indicates the range of the pressure-coefficient 5.3 1.3 cm1/GPa 400

LO (GaP) ω LO (cm-1)

380 360

LO (InP) LO (bulk InP)

340

Ga 0.5In0.5P 320

0

200

400

600

800

1000

T (K)

Figure 4.17 GaP- and InP-like LO phonon frequencies versus temperature T for Ga0.5In0.5P. The experimental data are taken from Shealy and Wicks [37]. The bulk InP data are also taken from Adachi [35]

The GaP- and InP-like LO phonon frequencies versus temperature T for Ga0.5In0.5P are plotted in Figure 4.17. The experimental data were measured by Raman spectroscopy [37]. The bulk InP vLO(T) values which were calculated from Equation (4.7) with vLO(0) ¼ 348.3 cm1, a ¼ 2.8 102 cm1/K and b ¼ 420 K are also shown [35]. The temperature variation in GaxIn1xP is found to be nearly the same as that in InP. The pressure dependence of the GaP- and GaAs-like LO and TO data for GaP0.11As0.89 is shown in Figure 4.18. The experimental data are taken from Galtier et al. [38]. The solid lines represent the bulk LO and TO values versus p for GaP and GaAs taken from Adachi [35]. The GaP0.11As0.89 data are found to be very similar to those for GaP. (c) II–VI semiconductor alloy The temperature variations of the LO and TO phonon frequencies vLO and vTO for c-ZnxCd1xSe are shown in Figure 4.19. The experimental data are taken from Valakh et al. [39]. The LO phonons in c-ZnxCd1xSe exhibit one-mode behavior, while the

116

PROPERTIES OF SEMICONDUCTOR ALLOYS 500 GaP0.11 As0.89

ω LO, TO (cm-1)

450

LO (bulk GaP)

400 350

LO (bulk GaAs) TO (bulk GaP)

300 TO (GaAs)

250

0

2

4

6

8

10

12

p (GPa)

Figure 4.18 Hydrostatic-pressure dependence of the GaP-like LO (solid circles) and TO phonon frequencies (open circles) in GaP0.11As0.89 at 85 K. The experimental data are taken from Galtier et al. [38]. The solid lines represent the bulk GaP and GaAs data taken from Adachi [35]

TO phonon branch is much more complicated. The resulting optical phonon behavior in c-ZnxCd1xSe is of the intermediate type, neither one-mode nor two-mode behavior. The experimental vLO versus T behavior in Figure 4.19 can be found in many ANB8N tetrahedral semiconductors. On the other hand, the effect of resonant interaction of the onephonon (TO) and two-phonon (2TA) states in c-ZnxCd1xSe [39] leads not only to the peculiar temperature dependence of intensity and line-shape of the bands, but also to the temperature

Figure 4.19 Temperature dependence of the LO and TO phonon frequencies vLO and vTO in c-ZnxCd1xSe. [Reprinted with permission from M. Y. Valakh et al., Phys. Status Solidi B 113, 635 (1982), Copyright (1982) Wiley–VCH]

LATTICE DYNAMIC PROPERTIES

117

300

LO (bulk ZnSe)

ω LO (cm -1)

280

260

LO (Zn 0.68 Cd 0.32 Se)

240

TO (bulk ZnSe)

220

200

0

2

4

6 p (GPa)

8

10

Figure 4.20 Hydrostatic-pressure dependence of the LO phonon frequency for Zn0.68Cd0.32Se layer grown on GaAs(100) measured at 300 K. The experimental data are taken from Li et al. [40]. The solid line shows the result calculated using Equation (4.8) (Zn0.68Cd0.32Se). The bulk ZnSe LO and TO phonon frequencies are obtained from Adachi [41]

shift of the phonon frequencies. The latter can be easily identified in Figure 4.19. The ordinary temperature shift in vLO takes place for x 0.75 for which the resonant interaction is small. When this interaction is significant (0.4 < x < 0.6), the phonon frequency vTO exhibits anomalous dependence on temperature; i.e. at x ¼ 0.50 and 0.58 vTO is practically unchanged over a wide temperature range from 100 to 450 K (Figure 4.19). This is due to the strengthening of anharmonic coupling with increasing temperature and, as a result, to the stronger repulsion effect of the TO and 2TA bands [39]. The pressure dependence of vLO for Zn0.68Cd0.32Se layer on GaAs(100) is shown in Figure 4.20. The Raman spectra were recorded up to 7 GPa [40]. The solid line represents the experimental data (vLO in cm1, p in GPa) vLO ðpÞ ¼ 241:07 þ 4:066p

ð4:8Þ

Also shown in Figure 4.20 are the experimental results for ZnSe [41] (vLO,TO in cm1, p in GPa) vLO ðpÞ ¼ 251:9 þ 3:44p0:02p2

ð4:9aÞ

vTO ðpÞ ¼ 204:2 þ 4:98p0:07p2

ð4:9bÞ

The pressure dependence of the ZnSe-like LO and TO phonon frequencies for MBE-grown ZnSe0.96Te0.04 layer is shown in Figure 4.21. The optical phonon frequencies were obtained by

118

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.21 Hydrostatic-pressure dependence of the ZnSe-like LO and TO phonon frequencies for ZnSe0.96Te0.04 at 300 K. [Reprinted with permission from C. S. Yang et al., Phys. Rev. B 59, 8128–8131 (1999). Copyright (1999) American Physical Society]

Raman scattering and FTIR measurements under pressures of up to 20 GPa [42]. Both ZnxCd1xSe (Figure 4.19) and ZnSexTe1x exhibit an intermediate-mode behavior (Table 4.5). In addition to the usual ZnSe-like LO and TO modes, a new LO–TO phonon pair can therefore be identified inside the reststrahlen band in ZnSexTe1x [25]. The ZnSe-like LO phonon frequency in Figure 4.21 can be approximated as (vLO in cm1, p in GPa) vLO ðpÞ ¼ 250 þ 3:3p

ð4:10Þ

On the other hand, the ZnSe-like TO phonon frequency exhibits anomalous dependence on p, i.e. it increases almost linearly up to 3 GPa and tends to show a saturated value of 225 cm1 for p > 3 GPa. There have been many Raman peaks observed in ZnSexTe1x for 0 < x < 1.0 between the ZnSe-like LO and TO phonon frequency region. The anomalous pressure dependence of the ZnSe-like TO phonon frequency may be correlated with this fact [42]. Raman scattering has been used to investigate anharmonicity and disorder-induced effects in MBE-BexZn1xSe/GaAs(100) epilayers [43]. The anharmonicity is found to be higher in BexZn1xSe than in ZnSe, increasing with compositional disorder. In conclusion of this section, the temperature and pressure coefficients of the longwavelength optical phonon frequencies dvop/dT (or v1 op dvop =dT ¼ d lnvop =dT) and dvop/ dp (or v1 op dvop =dp ¼ d lnvop =dp) in alloys of exhibiting one-mode behavior can be simply estimated from the linear interpolation between the endpoint values. In the case of two-mode (three- or four-mode) behavior in group-IV binaries and in III–V and II–VI ternaries (quaternaries), the temperature and pressure coefficients of the endpoint material values can be used, to a first approximation, as those for each phonon mode. For example, in an AxB1xC alloy, the temperature coefficient of the AC-like (BC-like) LO phonon frequency is the same as that of the bulk material AC (BC). These are schematically shown in Figure 4.22. A variety of the endpoint material data can be found in Adachi [33, 35, 41].

LATTICE DYNAMIC PROPERTIES

119

LO (AC) LO dωop /dT, dωop /dp

TO (AC)

TO

LO (BC) TO (BC) AxB1-xC

(a) one-mode 0

0.2

0.4

(b) two-mode 0.6

0.8

1.0 0

x

0.2

0.4

0.6

0.8

1.0

x

Figure 4.22 Schematic representations of the composition dependence of the temperature and pressure coefficients, dvop/dT and dvop/dp, in an alloy of composition AxB1xC (solid lines). The solid and open circles represent the endpoint binary data. The dependence of vop on x is also schematically shown by the dashed lines. The schemes represented by the solid lines can also be used for estimating mode Gr€ uneisen parameters and PDPs

€ 4.3 MODE GRUNEISEN PARAMETER The anharmonic properties of solids are customarily described in terms of the Gr€uneisen parameter g. As a measure of the volume dependence of the phonon frequency ni(q) of the ith mode, the mode Gr€ uneisen parameter g i(q) can be defined by g i ðqÞ ¼

d½lnni ðqÞ V dni ðqÞ ¼ d½lnV ni ðqÞ dV

ð4:11Þ

where V is the crystal volume. The mode Gr€ uneisen parameters for the long-wavelength (q ¼ 0) phonons in some non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Tables 4.5 and 4.6 of Adachi [31]. Figure 4.23 shows the g parameters for (a) SiSi, (b) SiGe and (c) GeGe modes in SixGe1x. The experimental data are taken from Sui et al. [32]. The Si and Ge values are also taken from Adachi [33]. The SiSi (GeGe) mode parameter slightly decreases (increases) with increasing x, while the SiGe mode parameter is nearly independent of x. The LO and TO phonon g parameters versus x for AlxGa1xAs are plotted in Figure 4.24. The alloy data are taken from Holtz et al. [36]. The binary data are also taken from Adachi [35]. These data scatter relatively largely, but show no strong dependence on x. They fall in the range g LO,TO ¼ 1.1 0.3, as indicated by the vertical bar. Figure 4.25 plots the mode Gr€ uneisen parameter g versus x for c-GaNxAs1x. The experimental data are taken from G€ ungerich et al. [44]. These authors used the pressure-dependent shift of the GaAs-like local vibrational mode to calculate the

120

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.6 γ

1.4 1.2 SixGe1-x

1

(a) Si-Si

0.8 1.6 γ

1.4 1.2 1

(b) Si-Ge

0.8 1.6 γ

1.4 1.2 1

(c) Ge-Ge

0.8 0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.23 Mode Gr€uneisen parameters g versus x for (a) SiSi, (b) SiGe and (c) GeGe phonon pairs in SixGe1x at 300 K. The experimental data are taken from Sui et al. [32]. The endpoint elemental data are also taken from Adachi [33]

anharmonicity of the GaN bond potential and qualitatively confirmed the simple picture in which the GaN bonds are significantly overstretched in Ga(N, As) with respect to their equilibrium length realized in GaN. Finally, the composition dependence of the mode Gr€uneisen parameter in various semiconductor alloys can be estimated, to a first approximation, from the scheme shown in Figure 4.22. Using an AxB1xC alloy that exhibits the two-mode behavior as an example, the AC-like LO phonon mode has the same Gr€ uneisen parameter as that of AC, irrespective of x. Similarly, the BC-like LO phonon mode has the same Gr€uneisen parameter as that of BC 2.1 1.8

AlxGa1-x As

1.5 γ

1.2 0.9

LO (AlAs) TO (AlAs) LO (GaAs) TO (GaAs)

0.6 0.3 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.24 Mode Gr€uneisen parameter g versus x for AlxGa1xAs at 300 K. The experimental data are taken from Holtz et al. [36]. The endpoint binary data are also taken from Adachi [35] (solid and open squares). The vertical bar indicates the range of g LO,TO ¼ 1.1 0.3

LATTICE DYNAMIC PROPERTIES

121

2.1 1.8

c-GaNx As1-x

γ

1.5 1.2 0.9 0.6

LO (GaAs) TO (GaAs)

0.3 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.25 Mode Gr€uneisen parameter g versus x for c-GaNxAs1x at 300 K. The experimental data are taken from G€ungerich et al. [44]

(Figure 4.22(b)). The endpoint g values for some non-alloyed group-IV, III–V and II–VI semiconductors can be found in Adachi [31,33,35,41].

4.3.1 Phonon Deformation Potential Strain- or stress-induced shift of the phonon frequency can be explained by the PDP [31]. The PDPs for some non-alloyed group-IV, III–Vand II–VI semiconductors are summarized in Adachi [31, 33, 35, 41]. A very few data have, however, been reported on alloy materials. This necessitates the use of some sort of an interpolation scheme. The interpolation scheme in Figure 4.22 may be the simplest and most reliable way to estimate alloy PDP values. Indeed, the GaN- and AlN-like E2 (high) phonon modes in w-AlxGa1xN have the same PDPs as the relevant endpoint binary values (w-GaN and w-AlN), respectively. [45]. The strain («)-induced shift of the LO phonon frequency can now be given by C12 S12 DvLO « ¼ vLO K12 ðLOÞ K11 ðLOÞ « ¼ vLO K12 ðLOÞ þ K11 ðLOÞ « C11 S11 þ S12 ð4:12Þ where Kij is the dimensionless PDP and Cij (Sij) is the elastic stiffness (compliance) constant. The Kij is usually defined, using p and q, as [31] K11 ¼

p ; v2LO

K12 ¼

q v2LO

ð4:13Þ

Equation (4.12) can, then, be rewritten as DvLO « ¼

1 C12 1 S12 qðLOÞ pðLOÞ « ¼ qðLOÞ þ pðLOÞ « b« ð4:14Þ vLO vLO C11 S11 þ S12

The b versus x data for SixGe1x are shown in Figure 4.26. The experimental data are taken from Lockwood and Baribeau [46] (open circles), Stoehr et al. [47] (open squares),

122

PROPERTIES OF SEMICONDUCTOR ALLOYS

b (cm-1)

-300 -600 -900 -1200

(a) Si-Si

b (cm-1)

-1500 -300 -600 -900 -1200

(b) Si-Ge

b (cm-1)

-1500 0 -300

(c) Ge-Ge

-600 -900 -1200

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.26 Optical-phonon strain-shift coefficient b versus x for SixGe1x at 300 K. The experimental data are taken from Lockwood and Baribeau [46] (open circles), Stoehr et al. [47] (open squares), Wong et al. [48] (open triangles) and Pezzoli et al. [49] (solid circles). The solid lines represent the linear leastsquares fit of these data

Wong et al. [48] (open triangles) and Pezzoli et al. [49] (solid circles). It can be seen that the SiGe and GeGe modes gradually decrease with increasing x, while the SiSi mode is nearly independent of x. However, Reparaz et al. [50] were unable to observe any clear composition dependence of the Si-like, Ge-like and SiGe modes in SixGe1x between x ¼ 0 and 0.6. The GaP- and GaAs-like LO-phonon coefficients b for GaPxAs1x are shown in Figure 4.27. The experimental data correspond to those for the (001) biaxial strain [51]. A much higher frequency shift of the GaAs-like mode than that of the GaP-like mode can be seen, suggesting

0 GaPx As1-x b (cm-1)

-300 LO (GaP)

-600 LO (GaAs)

-900 -1200

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.27 GaP- and GaAs-like LO-phonon strain-shift coefficients b versus x for GaPxAs1x at 300 K. The experimental data are taken from Armelles et al. [51]. The solid lines represent the linear leastsquares fit (in cm1): b ¼ 308–437x (GaP-like) and 513–1069x (GaAs-like)

LATTICE DYNAMIC PROPERTIES

123

that the biaxial strain is not accommodated in the same way by the two types of bonds in GaPxAs1x.

REFERENCES [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32]

C. W. Myles, Phys. Rev. B 28, 4519 (1983). S. Baroni, S. de Gironcoli, and P. Giannozzi, Phys. Rev. Lett. 65, 84 (1990). J. A. Kash, J. M. Hvam, J. C. Tsang, and T. F. Kuech, Phys. Rev. B 38, 5776 (1988). G. P. Srivastava, The Physics of Phonons. Adam Hilger, Bristol, (1990). I. F. Chang and S. S. Mitra, Adv. Phys. 20, 359 (1971). I. F. Chang and S. S. Mitra, Phys. Rev. 172, 924 (1968). A. Mascarenhas, H. M. Cheong, M. J. Seong, and F. Alsina, in Spontaneous Ordering in Semiconductor Alloys (edited by A. Mascarenhas), Kluwer Academic, New York, 2002, p. 391. F. Pezzoli, L. Martinelli, E. Grilli, M. Guzzi, S. Sanguinetti, M. Bollani, H. D. Chrastina, G. Isella, H. von K€anel, E. Wintersberger, J. Stangl, and G. Bauer, Mater. Sci. Eng. B 124–125, 127 (2005). J. C. Tsang, V. P. Kesan, J. L. Freeouf, F. K. LeGoues, and S. S. Iyer, Phys. Rev. B 46, 6907 (1992). M. Melendez-Lira, J. Menendez, W. Windl, O. F. Sankey, G. S. Spencer, S. Sego, R. B. Culbertson, A. E. Bair, and T. L. Alford, Phys. Rev. B 54, 12866 (1996). B.-K. Yang, M. Krishnamurthy, and W. H. Weber, J. Appl. Phys. 84, 2011 (1998). L. V. Kulik, C. Guedj, M. W. Dashiell, J. Kolodzey, and A. Hairie, Phys. Rev. B 59, 15753 (1999). H. Harima, T. Inoue, S. Nakamura, H. Okumura, Y. Ishida, S. Yoshida, T. Koizumi, H. Grille, and F. Bechstedt, Appl. Phys. Lett. 74, 191 (1999). A. Tabata, J. R. Leite, A. P. Lima, E. Silveira, V. Lemos, T. Frey, D. J. As, D. Schikora, and K. Lischka, Appl. Phys. Lett. 75, 1095 (1999). K. Torii, N. Usukura, A. Nakamura, T. Sota, S. F. Chichibu, T. Kitamura, and H. Okumura, Appl. Phys. Lett. 82, 52 (2003). B. Jusserand, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 30. Z. C. Feng, S. Perkowitz, R. Rousina, and J. B. Webb, Can. J. Phys. 69, 386 (1991). M. H. Brodsky, G. Lucovsky, M. F. Chen, and T. S. Plaskett, Phys. Rev. B 2, 3303 (1970). S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP. John Wiley & Sons, Ltd, New York, 1992. T. Sugiura, N. Hase, Y. Iguchi, and N. Sawaki, Jpn. J. Appl. Phys. 37, 544 (1998). R. Manor, O. Brafman, and R. F. Kopf, Phys. Rev. B 56, 3567 (1997). G. Lucovsky, E. Lind, and E. A. Davis, in II–VI Semiconducting Compounds (edited by D. G. Thomas), Benjamin, New York, 1967, p. 1150. J. Baars and F. Sorger, Solid State Commun. 10, 875 (1972). M. P. Volz, F. R. Szofran, S. L. Lehoczky, and C. -H. Su, Solid State Commun. 75, 943 (1990). T. R. Yang and C. C. Lu, Physica B 284–288, 1187 (2000). R. G. Alonso, E.-K. Suh, A. K. Ramdas, N. Samarth, H. Luo, and J. K. Furdyna, Phys. Rev. B 40, 3720 (1989). O. Pages, T. Tite, D. Bormann, O. Maksimov, and M. C. Tamargo, Appl. Phys. Lett. 80, 3081 (2002). O. Pages, M. Ajjoun, T. Tite, D. Bormann, E. Tournie, and K. C. Rustagi, Phys. Rev. B 70, 155319 (2004). D. Wang, D. Huang, C. Jin, X. Liu, Z. Lin, J. Wang, and X. Wang, J. Appl. Phys. 80, 1248 (1996). H. Makino, H. Sasaki, J. H. Chang, and T. Yao, J. Cryst. Growth 214/215, 359 (2000). S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. Z. Sui, H. H. Burke, and I. P. Herman, Phys. Rev. B 48, 2162 (1993).

124

PROPERTIES OF SEMICONDUCTOR ALLOYS

[33] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [34] J. Jimenez, E. Martın, A. Torres, and J. P. Landesman, Phys. Rev. B 58, 10463 (1998). [35] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [36] M. Holtz, M. Seon, O. Brafman, R. Manor, and D. Fekete, Phys. Rev. B 54, 8714 (1996). [37] J. R. Shealy and G. W. Wicks, Appl. Phys. Lett. 50, 1173 (1987). [38] P. Galtier, J. Chevallier, M. Zigone, and G. Martinez, Phys. Rev B 30, 726 (1984). [39] M. Y. Valakh, M. P. Lisitsa, G. S. Pekar, G. N. Polysskii, V. I. Sidorenko, and A. M. Yaremko, Phys. Status Solidi B 113, 635 (1982). [40] W. S. Li, Z. X. Shen, D. Z. Shen, and X. W. Fan, J. Appl. Phys. 84, 5198 (1998). [41] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [42] C. S. Yang, W. C. Chou, D. M. Chen, C. S. Ro, J. L. Shen, and T. R. Yang, Phys. Rev. B 59, 8128 (1999). [43] L. Y. Lin, C. W. Chang, W. H. Chen, Y. F. Chen, S. P. Guo, and M. C. Tamargo, Phys. Rev. B 69, 075204 (2004). [44] M. G€ungerich, P. J. Klar, W. Heimbrodt, J. Koch, W. Stolz, M. P. Halsall, and P. Harmer, Phys. Rev. B 71, 075201 (2005). [45] A. Sarua, M. Kuball, and J. E. Van Nostrand, Appl. Phys. Lett. 85, 2217 (2004). [46] D. J. Lockwood and J.-M. Baribeau, Phys. Rev. B 45, 8565 (1992). [47] M. Stoehr, D. Aubel, S. Juillaguet, J. L. Bischoff, L. Kubler, D. Bolmont, F. Hamdani, B. Fraisse, and R. Fourcade, Phys. Rev. B 53, 6923 (1996). [48] L. H. Wong, C. C. Wong, J. P. Liu, D. K. Sohn, L. Chan, L. C. Hsia, H. Zang, Z. H. Ni, and Z. X. Shen, Jpn. J. Appl. Phys. 44, 7922 (2005) . [49] F. Pezzoli, E. Bonera, E. Grilli, M. Guzzi, S. Sanguinetti, D. Chrastina, G. Isella, H. von K€anel, E. Wintersberger, J. Stangl, and G. Bauer, J. Appl. Phys. 103, 093521 (2008). [50] J. S. Reparaz, A. Bernardi, A. R. Gon~i, M. I. Alonso, and M. Garriga, Appl. Phys. Lett. 92, 081909 (2008). [51] G. Armelles, M. J. Sanjuan, L. Gonzalez, and Y. Gonzalez, Appl. Phys. Lett. 68, 1805 (1996).

5 Collective Effects and Some Response Characteristics 5.1 PIEZOELECTRIC CONSTANT 5.1.1 General Considerations A crystal with a center of symmetry cannot be piezoelectric [1]. Thus, the diamond-type crystals (diamond, Si, Ge and a-Sn) cannot be piezoelectric. Tables 5.1 and 5.2 summarize the piezoelectric constants for some ANB8N tetrahedral semiconductors with cubic and hexagonal crystal structures, respectively. Note that the piezoelectric strain constant dij is connected reciprocally with the stress constant eik in the following manner dij ¼

X

eik Skj

ð5:1Þ

dik Ckj

ð5:2Þ

k

or, vice versa eij ¼

X k

where Skj (Ckj) is the elastic compliance (stiffness) constant [1].

5.1.2 Alloy Value Figure 5.1 shows the plot of e14 versus x for CxSi1x. The theoretical e14 value for 3C-SiC is 0.345 C/m2 [2]. However, no experimental e14 data for 3C-SiC has been reported. Similarly, SixGe1x will in principle have a nonzero e14 value at an ordered phase x 0.5. In the fully disordered group-IV semiconductor alloys (CxSi1x, SixGe1x, etc.), we have zero e14 values over the whole alloy range 0 x 1.0. Using the endpoint binary data in Table 5.2, the liner interpolation scheme provides a set of the piezoelectric constants eij for w-AlxGa1xN (in C/m2) e15 ðxÞ ¼ 0:330:15x

ð5:3aÞ

e31 ðxÞ ¼ 0:550:03x

ð5:3bÞ

e33 ðxÞ ¼ 1:12 þ 0:43x

ð5:3cÞ

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

126

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 5.1 Piezoelectric stress and strain constants, e14 and d14, for some cubic group-IV, III–Vand II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt e14 (C/m2)

d14 (1012 m/V)

Diamond (d)a Si (d)a Ge (d)a Sn (d)a 3C-SiC (zb)

0 0 0 0 0.345b

0 0 0 0 1.35b

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

1.04b 0.36b 1.13b 0.06b 0.23b 0.068 0.61b 0.10 0.16 0.126 0.71b 0.083 0.045 0.071

System

Material

IV

III–V

II–VI

a b

MgO (rs)a ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs)a CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

0 0.147 0.049 0.028 0 0.37b 0.27b 0.0335 0.14b 0.058b 0.029b

9.7b 3.9b 1.7 6.4b 1.42 2.7 2.92 1.80 1.14 2.4 0 3.18 1.10 0.91 0 1.68 5.3b 2.6b 1.4b

Principally showing no piezoelectricity Estimated or calculated

The piezoelectric properties of ordered and disordered IIIN alloys have been theoretically studied by several authors [3,4]. The piezoelectric constant e33 versus x for w-GaxIn1xN is reproduced in Figure 5.2 [4]. The solid line shows the x dependence of e33 for disordered w-GaxIn1xN, while the solid circles refer to ordered values. Four ordered structures, all exhibiting ordering along the c axis, will be considered. The first structure is denoted 1 1 and consists of a single Ga plane alternating with a simple In plane. This structure has also been studied by Bernardini and Fiorentini [3] and has an overall composition x ¼ 0.5. The second structure, denoted 2 2, also has an overall composition of 50 at% but

COLLECTIVE EFFECTS AND SOME RESPONSE CHARACTERISTICS

127

Table 5.2 Piezoelectric stress and strain constants eij and dij for some hexagonal group-IV, III–V and II–VI semiconductors. w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)) System

eij (C/m2)

Material

dij (1012 m/V)

e31

e15 IV

2H-SiC (w)

0.08a

III–V

BN (h)b AlN (w) GaN (w) InN (w)

0 0.48 0.33c

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

e33

d15

d31

d33

0.2a

0.37 0.118 0.183 0.138

0 0.58 0.55 0.41c

0 1.55 1.12 0.81c

0.051 0.62 0.238 0.262 0.160

0.092 0.96 0.265 0.385 0.347

0 4.07 3.1

0 2.65 1.9

0 5.53 3.7 4.7

8.3 4.37 11.91 10.51

0.12 5.12 2.14 5.09 3.92

0.24 12.3 3.66 9.71 7.84

Assuming that the 2H-SiC values are the same as those for 6H-SiC within experimental error Principally showing no piezoelectricity c Estimated or calculated a b

e14 (C/m2)

0

CxSi1-x

-0.1

Disordered alloy

Ordered alloy

-0.2 -0.3

3C-SiC

-0.4 -0.5

0

0.2

0.4

x

0.6

0.8

1.0

Figure 5.1 Piezoelectric stress constant e14 versus x for CxSi1x. The open circles show the endpoint elemental data (e14 ¼ 0), while the solid circle refers to the theoretical 3C-SiC (x ¼ 0.5) value

Figure 5.2 Theoretical piezoelectric stress constant e33 versus x for w-GaxIn1xN. The solid line shows the disordered alloy values, while the solid circles plot the ordered values. [Reprinted with permission from A. Al-Yacoub, L. Bellaiche, and S.-H. Wei, Phys. Rev. Lett. 89, 7601–7604 (2002). Copyright (2002) American Physical Society]

128

PROPERTIES OF SEMICONDUCTOR ALLOYS

differentiates itself from the 1 1 structure by exhibiting two pure Ga planes alternating with two pure In planes. The third (respectively, fourth) structure exhibits a succession of three (respectively, one) Ga and one (respectively, three) In planes. Consequently, it is denoted as 3 1 (respectively, 1 3) while having a Ga composition of 75 at% (respectively, 25 at%). The theoretical results in Figure 5.2 indicate that the atomic ordering can have a large effect on the piezoelectricity and that e33 of disordered alloys is nearly linear with respect to x. The simple linear interpolation scheme, using the endpoint binary data in Table 5.2, provides e33 for w-GaxIn1xN (in C/m2) e33 ðxÞ ¼ 0:81 þ 0:31x

ð5:4Þ

Equation (5.4) indicates an increase in e33 with increasing x, in direct contrast to that obtained in Figure 5.2 [4]. Figure 5.3 shows the piezoelectric constant e14 as a function of x for GaxIn1xAs. The experimental data are taken from Sanchez-Rojas et al. [5] (solid circles), Chan et al. [6] (open square) and Izpura et al. [7] (open triangle). The solid line is obtained from the linear interpolation scheme between the endpoint data (open circles). It can be seen from Figure 5.3 that e14 passes through zero at x 0.2 while undergoing a reversal in sign. The experimental data are slightly larger than the linearly interpolated values. 0.08

e14 (C/m2)

0.04 0 -0.04 -0.08 Gax In1-x As

-0.12 -0.16 -0.20

0

0.2

0.4

x

0.6

0.8

1.0

Figure 5.3 Piezoelectric stress constant e14 versus x for GaxIn1xAs. The experimental data are taken from Sanchez-Rojas et al. [5] (solid circles), Chan et al. [6] (open square) and Izpura et al. [7] (open triangle). The solid line represents the linearly interpolated result between the endpoint binary data

No experimental data on alloy eij values have been reported, except for GaxIn1xAs (Figure 5.3). The piezoelectric constants e14 for AlxGa1xAs and GaxIn1xPyAs1y/InP in Figure 5.4 have been calculated from Equations (A.4) and (A.6), respectively, and can be given by e14 ðxÞ ¼ 0:23 þ 0:07x

ð5:5Þ

e14 ðyÞ ¼ 0:05 þ 0:15y0:18y2

ð5:6Þ

for AlxGa1xAs and

for GaxIn1xPyAs1y/InP.

COLLECTIVE EFFECTS AND SOME RESPONSE CHARACTERISTICS 0

129

0

e14 (C/m2)

(a) AlxGa1-x As -0.05

-0.05

-0.10

-0.10

-0.15

-0.15

-0.20

-0.20 (b) Ga xIn1-xPyAs1-y /InP

-0.25 0

0.2 0.4 0.6 0.8 1.0 x

-0.25 0

0.2 0.4 0.6 0.8 1.0 y

Figure 5.4 Piezoelectric stress constant e14 versus x or y for (a) AlxGa1xAs and (b) GaxIn1x PyAs1y/InP calculated from the linear interpolation scheme. The open circles show the endpoint binary data

€ 5.2 FROHLICH COUPLING CONSTANT 5.2.1 General Considerations The theory of Fr€ ohlich interaction in alloys of multi-mode phonon behaviors is very complex. Simply, it is possible to assume that there is a value for the Fr€ohlich coupling constant aF for each phonon mode given by pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ h=2mac vLO 1 1 e2 = 1 aF ¼ 2 «¥ «s vLO h

ð5:7Þ

where e is the electron charge, mac is the electron effective mass (conductivity mass), vLO is the LO phonon frequency and «¥ and «s are the high-frequency and static dielectric constants, respectively. The final alloy aF value can be obtained from the weighted average of each mode (i.e. Equation (5.7)). Nash et al. [8] discussed the Fr€ ohlich interaction in alloys of two-mode behavior based on a MREI model. They found that the electron–phonon coupling in In0.53Ga0.47As is much weaker for the InAs-like mode than for the GaAs-like mode. The primary reason for this was considered to be the coupling of the LO distortions by the macroscopic electric field. A theory of the Fr€ ohlich interaction in semiconductor alloys has also been proposed by several authors [9,10].

5.2.2 Alloy Value Table 5.3 summarizes the Fr€ ohlich coupling constant aF for some non-alloyed group-IV, III–V and II–VI semiconductors. The simplest way to obtain the alloy value is to use the linear interpolation scheme using the endpoint data in Table 5.3.

130

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 5.3 Fr€ohlich coupling constant aF for some group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite; rs ¼ rocksalt System

Material

aF

System

Material

aF

IV

Diamond (d)a Si (d)a Ge (d)a Sn (d)a 3C-SiC (zb)

0 0 0 0 0.256

II–VI

III–V

AlN (w) AlAs (zb) AlSb (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

0.65 0.126 0.023 0.48 0.201 0.068 0.025 0.24 0.15 0.0454 0.022

ZnO (w) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (w) CdSe (w) CdTe (zb)

1.19 0.63 0.432 0.332 0.75 0.514 0.46 0.35

a

Principally showing no Fr€ohlich coupling interaction

αF

The x dependence of aF for CxSi1x is shown in Figure 5.5. The Fr€ohlich coupling constant aF is strongly dependent on the ionic polarization of the crystal, which is related to the static and high-frequency dielectric constants «s and «¥. Note that «s is equal to «¥ in such diamondtype crystals. Thus, no Fr€ ohlich coupling occurs in diamond-type crystals (aF ¼ 0, see Equation (5.7)). 0.35 0.30 0.25 0.20 0.15 0.10 0.05 0

Cx Si1-x 3C-SiC

Ordered alloy

0

0.2

0.4

Disordered alloy

x

0.6

0.8

1.0

Figure 5.5 Fr€ohlich coupling constant aF versus x for CxSi1x. The open circles show the endpoint elemental data, while the solid circle refers to the experimental 3C-SiC (x ¼ 0.5) value

The aF value of 3C-SiC is 0.256 [11]. This means that the bond polarity of SiC resembles that of III–V and II–VI semiconductors (aF 6¼ 0) rather than that of Si or diamond (aF ¼ 0). Similarly, an alloy of SixGe1x will have a nonzero aF value near the ordered phase x 0.5, although this has never been confirmed experimentally. In the fully disordered alloys (CxSi1x, SixGe1x, etc.), a value of aF ¼ 0 can be expected over the whole alloy range 0 x 1.0.

COLLECTIVE EFFECTS AND SOME RESPONSE CHARACTERISTICS

131

0.20

αF

0.15

Gax In1-x Py As1-y /InP

0.10 0.05 0 0

0.2

0.4

0.6

0.8

1.0

y

Figure 5.6 Fr€ohlich coupling constant aF versus y for GaxIn1xPyAs1y/InP. The solid line shows the linear interpolation result of Equation (A.6), which can be successfully approximated by the quadratic expression shown in Equation (5.8). The open circle shows the InP data

The linearly interpolated aF value, obtained using Equation (A.6), is shown versus y for GaxIn1xPyAs1y/InP in Figure 5.6. This plot gives very weak upward bowing and can be expressed as aF ðyÞ ¼ 0:056 þ 0:107y0:013y2

ð5:8Þ

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] A. P. Mirgorodsky, M. B. Smirnov, E. Abdelmounıˆm, T. Merle, and P. E. Quintard, Phys. Rev. B 52, 3993 (1995). [3] F. Bernardini and V. Fiorentini, Phys. Rev. B 64, 085207 (2001); erratum, ibid. 65, 129903 (2002). [4] A. Al-Yacoub, L. Bellaiche, and S.-H. Wei, Phys. Rev. Lett. 89, 057601 (2002). [5] J. L. Sanchez-Rojas, A. Sacedon, F. Gonzalez-Sanz, E. Calleja, and E. Mu~ noz, Appl. Phys. Lett. 65, 2042 (1994). [6] C. H. Chan, Y. F. Chen, M. C. Chen, H. H. Lin, and G. J. Jan, J. Appl. Phys. 84, 1595 (1998). [7] I. Izpura, J. F. Valtue~na, J. L. Sanchez-Rojas, A. Saced on, E. Calleja, and E. Mu~ noz, Solid-State Electron. 40, 463 (1996). [8] K. J. Nash, M. S. Skolnick, and S. J. Bass, Semicond. Sci. Technol. 2, 329 (1987). [9] R. Zheng and M. Matsuura, Phys. Rev. B 59, 15422 (1999). [10] X. X. Liang and S. L. Ban, J. Lumin. 94–95, 781 (2001). [11] E. Kartheuser, in Polarons in Ionic Crystals and Polar Semiconductors (edited by J. T. Devreese), North-Holland, Amsterdam, 1972, p. 717.

6 Energy-band Structure: Energy-band Gaps 6.1 INTRODUCTORY REMARKS 6.1.1 Quasi-cubic Band Model The review in this chapter is concerned with the most important band-gap energies as a function of alloy composition. They are: E0, E0 þ D0, E1, E1 þ D1, E2, EgX , EgL , etc., and some of these gaps are shown in Figure 6.1 (see also Adachi [1]). In Figure 6.1, the fundamental absorption refers to band-to-band or to excitonic transitions. The fundamental absorption manifests itself by a rapid rise in absorption and can be used to determine the band-gap energy of semiconductors and insulators. In most semiconductors, the lowest direct band-gap transitions occur at the E0 edge, i.e. at the center of the BZ. Birman [2] discussed the relationship between the k ¼ 0 (G) CB and VB states of the wurtzite structure and the corresponding states of the zinc-blende structure. The essential difference between the potential that an electron experiences in an ideal wurtzite lattice and that in a zinc-blende lattice is the relatively small difference in ‘crystal field’ due to sites beyond the next nearest neighbors. Figure 6.2 shows the CB and VB states for (a) zinc-blende (Dso ¼ Dcr ¼ 0), (b) zinc-blende (Dso 6¼ 0, Dcr ¼ 0) and (c) wurtzite semiconductors at k ¼ 0. In the actual VB structure of a wurtzite crystal, the three VBs illustrated in Figure 6.2(c) can be thought of as arising from Figure 6.2(a) by the combined effect of both SO and crystal-field perturbations, while the wavefunction for each band may be written as a linear combination of px, py and pz and spin functions, provided the interaction of the G7 VB levels with the CB is neglected. This approach is known as the quasi-cubic model [3]. Under the SO interaction represented by the matrix element Dso and that of the crystal field represented by Dcr, the quasi-cubic model provides the difference in energies of the VBs DEBA ¼ E0B E0A

Dso þ Dcr ¼ 2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Dso þ Dcr 2 2 Dso Dcr 3 2

DECA ¼ E0C E0A

Dso þ Dcr þ ¼ 2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Dso þ Dcr 2 2 Dso Dcr 3 2

ð6:1aÞ

ð6:1bÞ

The lowest direct band-gap energies in wurtzite semiconductors can then be given by E0A, E0B and E0C, as shown in Figure 6.2(c). The lowest direct (E0) and lowest indirect gap energies (EgX , EgL ) for some group-IV, III–V and II–VI semiconductors are summarized in Table 6.1. Table 6.2 also lists the lowest direct Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

134

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 6.1 Electronic energy-band structure of Ge. The electronic states are labeled using the notation for the representations of the double group of the diamond structure. The main interband transitions are indicated by vertical arrows (at 300 K)

Zincblende Γ1

Wurtzite

Γ6

Γ7

E0 Γ15

E0A E0B

E0C

Γ9 (A)

Γ8 Γ7

(a) ∆so=∆cr=0

E0+∆0

∆so=∆0

(b) ∆cr=0

∆EBA

Γ7 (B) Γ7 (C)

∆ECA

(c) ∆so>0, ∆cr>0

Figure 6.2 Relationships between the VB splitting at the G point in the zinc-blende ((a) Dso ¼ Dcr ¼ 0, (b) Dso 6¼ 0, Dcr ¼ 0) and (c) wurtzite lattices (Dso 6¼ 0, Dcr 6¼ 0) and between the irreducible representations of the CB and VB in these lattices. (b) and (c) show the actual splitting found in the zinc-blende and wurtzite crystals, respectively

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

135

Table 6.1 E0, EgX and EgL for some cubic group-IV, III–V and II–VI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

II–VI

BN (zb) BP (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb) BeS (zb) BeSe (zb) BeTe (zb) MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnO (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

Estimated At 1.5 K c At 4.2 K d Calculated or estimated e Tentative assignment f Estimated from AlxGa1xP data g Grown on MgO(100) substrate a b

E0 (eV) 15.3 4.06 0.795 0.413b 7.4 7.9–11.40d 5 1.45e 5.2 3.91f 3.01 2.27 3.231g 2.76 1.43 0.72 0.56 1.35 0.359 0.17 > 5.5 5.6 4.1 7.8 4.45 4.0 3.4 3.17 3.726 2.721 2.27 2.16 2.46 1.675 1.51 0.04 0.08 0.15

EgX (eV)

EgL (eV)

5.50 1.12 0.852

7.26a 2.0 0.6657 0.092c 4.20

2.39 6.27 2.0 5.34 2.48 2.15 1.615 4.2d 2.261 1.911 1.05 3.0d 2.21 1.37 1.63

8.6d 3.57d 2.37 2.211 5.5d 2.63 1.72 0.76 5.8d 2.05 1.07 0.93

4–4.5 2.63 3.6d 3.2d 2.5d 5.14d 3.4 3.05 5.24d 4.37d 3.48d

3.8

136

PROPERTIES OF SEMICONDUCTOR ALLOYS

gaps E0A, E0B and E0C for some wurtzite-type group-IV, III–V and II–VI semiconductors. The Dso and Dcr values can be seen in Table 6.6 of Adachi [1].

6.1.2 Bowing Parameter In a conventional band-structure calculation, the electrons are assumed to be independent particles interacting with some average potential due to positively charged ions and valence electrons, at an equilibrium lattice constant a. Since the electron wavefunction in a strictly periodic function must be of the form exp(ikr)uk(r), where uk(r) is a periodic function which satisfies the periodic boundary conditions, it is convenient to compute electron energies E as a function of k. The computed energies are then drawn for various values of the wavevector lying along high symmetry lines in the first BZ (Figure 6.1). Though an alloy has no translational invariance, the VCA can recover it by replacing the potential by a periodic one, which is produced by ‘average’ atoms. For an AlxGa1xAs alloy, the potential is approximated by uVCA(r) ¼ xuAlAs(r) þ (1 x)uGaAs(r), which is periodic. The band-gap energy is a typical case exhibiting nonlinearity with respect to alloy composition. Van Vechten and Bergstresser [4] developed a physical model for obtaining the bowing parameter of E0 based on the Phillips’s dielectric theory of electronegativity [5]. The deviation from linearity is considered to be due to two terms involving ci, the intrinsic bowing parameter due to the VCA, and ce, the extrinsic bowing parameter due to aperiodicity in the alloy lattice c ¼ ci þ ce

ð6:2Þ 2 CA-B ,

i.e. to the square of the The extrinsic term ce can be taken to be proportional to electronegativity difference CA-B between the atoms A and B in an AxB1xC alloy.

6.1.3 Ordered Alloy As mentioned in Section 1.3.2, it has become evidence that many cubic semiconductor alloys can exhibit spontaneous ordering. For example, Ga0.5In0.5P, when grown under proper conditions, forms the CuPt-B ordered structure. In this structure, an alternate GaP/InP monolayer SL is formed along the h111i direction. The effects of atomic ordering lead to many interesting effects, such as the band-gap reduction, VB splitting and polarization dependence of the optical transitions [6]. The schematic energy-band diagram of the disordered zinc-blende and ordered CuPt-B structures at the G point, where the electronic states are labeled in Slater–Koster notation [7] is shown in Figure 6.3. The essential difference between the potential that an electron experiences in an ideal zinc-blende lattice and that in an ordered CuPt-B structure is the relatively small differences in ‘crystal field (Dscr )’ due to sites beyond the next nearest neighbors. The detailed differences in the energy bands then arise from the difference in the crystal field and also from the SL nature in ordered materials. These can be briefly summarized as follows [6]: 1. The lowest CB G4 in the CuPt-B structure corresponds to the CB G6 in the zinc-blende structure, whereas the upper CB G4 derives from the back-folded L-point CB minimum L6. Because of the same symmetry of these states their energies are shifted compared to those of

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

137

Table 6.2 E0a (a ¼ A, B or C) or related excitonic gap energy for some wurtzite group-IV, III–V and II–VI semiconductors at 300 K System

Material

IV III–V

2H-SiC AlN GaN InN BeO MgSe ZnO ZnS CdS CdSe CdTe

II–VI

a b

E0A (eV)

E0B (eV)

3.330a 6.2 3.420 0.70 10.6 4.1b 3.45 3.75 2.501 1.751 1.56b

E0C (eV)

3.428

3.40 3.78 2.516 1.771

3.55 3.87 2.579 2.176

At 4.2 K Estimated

the ordered Ga0.5In0.5P due to the level repulsion by a certain amount, the value of which increases with increasing order parameter h. This leads to a reduction in the gap between the upper VBs G5, G6 and the lowest CB G4, whereas the gap to the second lowest CB G4(L6) increases. 2. Due to reduction of symmetry with regard to the order direction ½111, the degeneracy of the j ¼ 3/2 states at the G point is lifted. The G5, G6 states correspond to the (3/2, 3/2) HH and the G4 state to the (3/2, 1/2) LH band. The VB splitting between the G5, G6(A) and G4(B) states again increases with increasing order parameter h. The VB SO split-off band G4(C) shows a rather weak dependence on the order parameter for the usual values of h < 0.5.

Disordered (Td) L1

Ordered (C3v)

L6 Γ1

Γ4 Γ6

Γ4 E0

Γ15

E0+∆0

E0A E0B

E0C

Γ8

Γ5, Γ6 (A) Γ4 (B)

∆so=∆0 Γ7

(a) ∆so=∆cr=0

(b) ∆cr=0

Γ4 (C) (c) ∆sso>0, ∆scr>0

Figure 6.3 Schematic energy-band diagram of the disordered zinc-blende and ordered CuPt-B structures at the G point. Note that the upper CB G4 in (c) derives from the back-folded L-point CB minimum L6 in (b)

138

PROPERTIES OF SEMICONDUCTOR ALLOYS

The triply degenerate G15 VB in Figure 6.3(a) is split into three states by the SO (Dsso ¼ Ds0 ) and crystal-field interactions (Dscr ). These three states can be described by the same model as that in Equation (6.1) by replacing Dso with Dsso and Dcr with Dscr . The VB splitting at the top of the VB for CuPt-B ordering can then be given by sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ s Dsso þ Dscr Dso þ Dscr 2 2 s s ð6:3aÞ Dso Dcr DEBA ðhÞ ¼ E0B ðhÞE0A ðhÞ ¼ 3 2 2 Ds þ Dscr þ DECA ðhÞ ¼ E0C ðhÞE0A ðhÞ ¼ so 2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ s Dso þ Dscr 2 2 s s Dso Dcr 3 2

ð6:3bÞ

The quantities that are experimentally accessible are DEBA(h), DECA(h) and Eg(h) ¼ E0A(h) for partially ordered alloys and for random alloys. These values can be used to derive Dsso ðhÞDsso ð0Þ ¼ Dsso ðhÞD0 ¼ h2 ½Dsso ð1ÞD0

ð6:4aÞ

Dscr ðhÞDscr ð0Þ ¼ Dscr ðhÞ ¼ h2 Dscr ð1Þ

ð6:4bÞ

DEg ðhÞ ¼ Eg ðhÞEg ð0Þ ¼ h2 DEg ð1Þ

ð6:4cÞ

where h ¼ 0 and 1 describe perfectly disordered (Dsso ð0Þ ¼ D0 and Dscr ð0Þ ¼ 0) and ordered materials, respectively, and DEg(1) represents the maximum band-gap reduction for perfectly ordered material. However, since perfectly ordered (h ¼ 1) samples are unavailable, and also the degree of the order parameter h of a given sample is not usually determined directly, Dsso ð1Þ, Dscr ð1Þ and DEg(1) cannot be found by this fitting procedure. Only the ratio j¼

DEg ð1Þ Dsso ð1ÞD0

ð6:5aÞ

DEg ð1Þ Dscr ð1Þ

ð6:5bÞ

z¼

can be determined from the measurement of DEBA(h), DECA(h) and Eg(h) ¼ E0A(h). On the other hand, if (Dsso ð1ÞD0 ), Dscr ð1Þ and DEg(1) were known independently (e.g. from theoretical calculation), then experimental values for DEBA(h), DECA(h) and Eg(h) could be used to derive h from the above equations. The maximum band-gap reduction for perfectly ordered Ga0.5In0.5P is reported to be 0.47 eV [8]. Perfectly ordered material has, of course, never been observed. In the most ordered Ga0.5In0.5P structure, the highest order parameter h is 0.6 [9] and the degree of ordering is nonuniform on the local scale. In Figure 6.4 the band-gap energy reduction DEg(h) has been plotted against the squared order parameter h2 for Ga0.5In0.5P. The experimental data are taken from Forrest et al. [10]. It has been established that DEg(h) increases almost linearly with increasing h2. The solid line in Figure 6.4 represents the relationship, DEg(h) ¼ 0.49h2 eV. From Equation (6.4c), the maximum band-gap reduction is found to be DEg(1) ¼ 0.49 eV for perfectly ordered Ga0.5In0.5P.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

139

Figure 6.4 Band-gap energy reduction DEg(h) against squared order parameter h2 for Ga0.5In0.5P. The experimental data are taken from Forrest et al. [10]. The solid line shows the relationship, DEg(h) ¼ 0.49h2 eV

6.2 GROUP-IV SEMICONDUCTOR ALLOY 6.2.1 Binary Alloy (a) CSi The indirect and direct gap energies EgX and E0 for diamond and Si, together with those for 3CSiC (x ¼ 0.5) are shown in Figure 6.5. The experimental data are taken from Table 6.1. The solid lines in Figure 6.5 show the best fit of these data using the parabolic expressions (in eV) EgX ðxÞ ¼ 1:12 þ 0:70x þ 3:68x2

ð6:6Þ

E0 ðxÞ ¼ 4:06 þ 2:12x þ 9:12x2

ð6:7Þ

There is, however, some ambiguity about the band-gap energies and band lineups in CxSi1x/Si heterostructures. The large tensile strain in pseudomorphic CxSi1x layers on Si is expected to strongly affect the band edges (see Section 9.1.2). The higher-lying CPs of supersaturated CxSi1x (x < 0.02) have become the origin of some controversy in the literature. Using ER and SE, Kissinger et al. [11] and Zollner et al. [12] found that the E1 gap in CxSi1x increases linearly with increasing x, as shown in Figure 6.6. The slopes in Figure 6.6 at 300 K give DE1 ¼ 35 meV/at%[C] and DE0 0 ¼ 7 meV=at%½C. On the other hand, Demkov and Sankey [13] argued that the band gaps of free-standing CxSi1x should decrease with increasing x. For strained pseudomorphic alloy, the lower of the two strain-split E1 energies should decrease even more. Additional weak structures in the SE spectra of CxSi1x and CxSiyGe1xx at 2.7 and 3.0 eV were, indeed, observed by Zollner et al. [12] and Lee et al. [14]. These structures were interpreted as previously unidentified optical transitions in the materials due to defects or C-related bands [14]. More recently, Zollner et al. [15] suggested

140

PROPERTIES OF SEMICONDUCTOR ALLOYS 18 15

CxSi1-x

Eg (eV)

E0

3C-SiC

12 9 6

E gX

3 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.5 Energies of the indirect gap EgX and direct gap E0 for diamond and Si at 300 K, together with those for 3C-SiC (x ¼ 0.5). The open circles represent the endpoint elemental data in Table 6.1. The solid lines show the best-fit results of these data using Equations (6.6) and (6.7)

that the new structures are actually interference fringes originating from the reflection of light at the alloy/substrate interface. (b) CGe Figure 6.7 shows the lowest indirect gap energies EgX and EgL versus x for CxGe1x. Kolodzey et al. [16] measured the optical absorption spectra of CxGe1x grown on Si(1 0 0) by MBE. Schrader et al. [17] also carried out optical absorption measurements on CxGe1x/Si deposited by hollow-cathode sputtering. The EgL values obtained from these studies are shown in Figure 6.7 by the open and solid circles. The linearly interpolated E0 and EgX values using

3.6 CxSi1-x

Eg (eV)

3.5 E1

3.4

E0'

3.3 T=80 K 300 K 3.2 0

0.3

0.6 0.9 x (at%)

1.2

1.5

Figure 6.6 Energies of the DE00 and E1 CPs versus x for CxSi1x at 300 K. The experimental data are taken from Kissinger et al. [11] (solid and open triangles) and Zollner et al. [12] (solid and open circles). The slopes shown by the solid lines give DE1 ¼ 35 meV/at%[C] and DE00 ¼ 7 meV=at%½C (at 300 K)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

141

1.5

E0

E gID (eV)

1.2

EgX

0.9

EgL

0.6

CxGe1-x

0.3 0

2

4

6

8

10

12

x (at%)

Figure 6.7 Energies of the lowest indirect gaps EgL and EgX and direct gap E0 versus x for CxGe1x at 300 K. The experimental data are taken from Kolodzey et al. [16] (open circles) and Schrader et al. [17] (solid circle). The solid triangles represent the endpoint elemental data in Table 6.1. The solid lines show the calculated results using data in Table 6.3

the endpoint data in Table 6.1 are shown by the solid lines. Table 6.3 summarizes the three main band-gap energies E0, EgX and EgL for CxGe1x. From these results, we can expect the EgX EgL crossover to occur at x 0.1. Extrapolation gives an EgL value of 7.26 eV for diamond. Table 6.3 Energies for some indirect and direct gaps in CxGe1x at 300 K. LF ¼ linear fit; LI ¼ linear interpolation Band Gap

Expression (eV)

Remark

EgL E0 EgX

0.66 þ 6.60x 0.795 þ 14.505x 0.852 þ 4.648x

LF LI LI

The higher-lying CPs, such as E1, E1 þ D1, E0 0 and E2, for CxGe1x have been determined using SE for x up to 0.03 [18]. These CPs are found to be roughly the same as those which do not contain C. (c) SiGe 1. Relaxed alloy—The binary alloy of Si and Ge provides a continuous series of materials with gradually varying physical properties. The physical properties of SixGe1x grown on Si have been under extensive study stimulated by their potential for use in various device applications. Due to the large lattice mismatch (Da/a 4 %), however, the critical layer thickness for pseudomorphic SixGe1x growth decreases drastically with increasing x [19]. The lattice constant of ‘relaxed,’ or in other words ‘unstrained’ SixGe1x, has been measured and showed to obey Vegard law (Section 1.4.3). The composition dependence of the fundamental absorption edge in SixGe1x was first determined by Braunstein et al. [20] using optical absorption and more recently by Weber

142

PROPERTIES OF SEMICONDUCTOR ALLOYS

and Alonso [21] using PL measurements. Figure 6.8(a) shows the results obtained by Braunstein et al. [20]. The crossing-over of the lowest-lying CB states from the L point to the X point (or D direction) is found at x 0.15. Thus, the conduction electron nature of SixGe1x changes from ‘Ge-like’ to ‘Si-like’ at x 0.15. The solid lines in Figure 6.8(a) represent the results calculated from the data in Table 6.4. 1.2

6 (a)

(E0)

1.1

E2 (Σ)

4

0.9

E gD (eV)

E gID (eV)

1.0

E gX

0.8

0.2

E2 (X)

E1+∆1

E0'

3

E0+∆0

0.4

0.6

0.8

E0

1

SixGe1-x 0

E1

2

E gL

0.7 0.6

E1'

5

(b) 1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

x

Figure 6.8 (a) Energies of the fundamental absorption edges EgL and EgX versus x for relaxed SixGe1x at 300 K. The experimental data are taken from Braunstein et al. [20]. (b) Energies of some CPs versus x for SixGe1x at 300 K. The solid circles in (a) and (b) represent the endpoint elemental data in Table 6.1 and Adachi [1]. The solid lines in (a) and (b) show the calculated results using the data in Table 6.4

The direct gap energies in relaxed SixGe1x have been determined using various measurement techniques, such as SE and ER. Table 6.4 summarizes the lowest direct and Table 6.4 Energies for some indirect and direct gaps in relaxed SixGe1x at 300 K. LI ¼ linear interpolation; QF ¼ quadratic fit Band Gap

Expression (eV)

Remark

EgL E0 EgX E0 þ D0 E1 E1 þ D1 E00 E2(X) E2(S) E10

0.66 þ 1.34x 0.795 þ 3.265x 0.852 0.032x þ 0.300x2 1.08 þ 3.05x 2.108 þ 1.134x þ 0.153x2 2.296 þ 1.070x þ 0.062x2 3.03 þ 0.32x 4.291 0.116x þ 0.084x2 4.406 0.005x þ 0.072x2 5.80 0.48x

LI LI QF LI a a a b b LI

a b

C. Pickering et al., Proc. SPIE 1985, 414 (1993) J. H. Bahng et al., J. Phys.: Condens. Matter 13, 777 (2001)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

143

higher-lying direct gap energies in relaxed SixGe1x alloy. Note that the E2 transitions in Si (and SixGe1x) occur not only along the h110i direction (S) but also near the X point (or D direction). All these CPs, including E0 and E0 þ D0, are plotted against x in Figure 6.8(b). Except for E00 and E2, the band-gap energies in SixGe1x are found to be fairly sensitive to x. 2. Strained alloy—The band structure of pseudomorphical SixGe1x epilayers on Si(100) substrates is drastically altered by the built-in strain or stress. The remarkable effect of the biaxial or uniaxial stress on the band structure is to split the HH (3/2, 3/2) and LH (3/ 2, 1/2) degeneracy at the G point (see Figure 8.1 in Adachi [1]). The biaxial tetragonal distortion can also shift and split the CB edge, for example, the sixfold degenerate CB minima at the X point or along D in bulk Si split into twofold and fourfold minima under [001] compressive strain [1]. The fundamental absorption edge of strained SixGe1x/Si(100) has been investigated by several authors using photocurrent [22] and PL [23,24]. These results are summarized in Figure 6.9. The heavy gray lines show the theoretical results obtained by People [25]. The experimental data agree well with the theoretical values.

1.2

1.1

E gL

E gID (eV)

1.0

E gX

0.9

0.8 HH & LH 0.7 SixGe1-x /Si(100) 0.6 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.9 Energies of the fundamental absorption edges EgL and EgX versus x for strained SixGe1x/Si (100) epilayer. The experimental data are taken from Lang et al. [22] (solid triangles, at 90 K), Dutartre et al. [23] (solid circles, at 90 K) and Liu et al. [24] (at 77 K, open circles). The light solid line shows the low-temperature values of relaxed SixGe1x epilayer. The heavy gray lines show the theoretical results of People [25]

144

PROPERTIES OF SEMICONDUCTOR ALLOYS

SE, ER and PR techniques have been used to determine the CP energies in strained SixGe1x/Si epilayers [26–30]. A decrease in the E1 energy with increasing x, compared with that observed in relaxed SixGe1x samples, has been reported [26,27]. On the other hand, Bahng et al. [29] reported an increase in the E1/(E1 þ D1), DE0 0 and E2 energies with increasing in-built strain in strained Si0.8Ge0.2/Si(1 0 0), where the strain was controlled by depositing different thickness of the Si0.8Ge0.2 epilayers from 35 to 350 nm. In the case of the externally applied uniaxial stress X||[0 0 1], the E1 energy in bulk Si decreased (increased) with increasing X for the light polarization E||X (E?X) used in the SE measurements [31]. Therefore, attention must be paid to analyzing the effects of in-built strain on the electronic energy-band structure of strained materials based on the standard DP theory [1]. 3. External perturbation effect—The temperature dependence of the fundamental absorption edge in relaxed SixGe1x alloy was measured by Braunstein et al. [20]. The experimental data were found to be essentially the same as those for bulk Si and Ge [1]. The temperature dependence of the higher-lying CPs in relaxed and strained SixGe1x has been measured by Humlıcek et al. [32] and Ebner et al. [30], respectively. The relaxed alloy data obtained are: dE1/dT (3 1) 104 eV/K and dE2/dT (2–4) 104 eV/K (x ¼ 0–1.0). All strainedalloy CP data also satisfactorily fitted the phenomenological formulas of Varshni and Vi~ na [1]. The influence of hydrostatic pressure on the ER spectra of relaxed SixGe1x alloy has been reported to be given by dE1/dp ¼ 7.8 1.6x meV/kbar and dE0 0 =dp ¼ 1:40:4x meV=kbar [33]. (d) GeSn The fundamental absorption edge in GexSn1x is expected to change from the Ge L6 indirect to the Sn G7 direct gap depending on x. The band structure near the direct–indirect transition region in relaxed or epitaxial GexSn1x films has been studied using optical absorption [34,35], SE [36,37] and PR [37]. Figure 6.10(a) shows the E0 and EgL energies versus x for nearly relaxed GexSn1x (1.0 > x 0.85) deposited on 10 nm thick relaxed Ge buffer layers on Si(100) substrates by MBE [34] and those obtained for epitaxial GexSn1x films (1.0 > x 0.86) deposited on Ge(100) substrates by rf magnetron sputtering [35]. Note that a-Sn (gray tin) is a zero gap semiconductor (i.e. semimetal) with degenerate valence and conduction bands at the center of the BZ. Thus, the lowest direct gap energy E0 (G8 þ ! G7) in a-Sn has a negative value (0.413 eV at 1.5 K, see Table 6.1). The solid lines in Figure 6.10(a) represent the quadratic fits of the experimental data. The resulting expressions are given in Table 6.5. These expressions predict that E0 and EgL become zero at x 0.67 and 0.25, respectively. GexSn1x should therefore be a semimetal at up to x 0.7. These expressions also predict that E0 and EgL cross at x 0.88. The interband transition energies in GexSn1x have been studied by D’Costa et al. [37]. Because of insufficient sensitivity of SE for energies below 1 eV, they carried out PR measurements at 15 K. Like E0 (Figure 6.10(a)), E0 þ D0, E1/(E1 þ D1), E00 and E2 decreased with increasing Sn concentration. From the quadratic fits of the 15 K data, they determined the bowing parameter of each CP. Introducing these parameters and binary data into Equation (A.17), we obtain the CP energies of GexSn1x at 300 K, as listed in Table 6.5. The numeric results of these expressions are shown in Figure 6.10(b).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

5

0.9

(a)

(b)

4

E0

0.6

E2

E gL E gD (eV)

E0,E gL (eV)

3 0.3 E gL

0

E0 ' E1+∆1

2

E1

1 E0 -0.3

0

0.2

0.4

0.6

0.8

E0+∆0

0

Ge x Sn 1-x -0.6

145

1.0

-1

E0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.10 (a) Energies of the lowest direct E0 (solid circles) and lowest indirect gap EgL (open circles) versus x for GexSn1x at 300 K. The experimental data are taken from He and Atwater [34] and de Guevara et al. [35]. (b) Energies of some CPs versus x for GexSn1x at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.5 Table 6.5 Energies for some indirect and direct gaps in GexSn1x at 300 K. QF ¼ quadratic fit Band Gap E0 EgL E0 þ D0 E1 E1 þ D1 E00 E2 a

Expression (eV) 0.413 0.617x þ 1.826x2 0.092 0.702x þ 1.275x2 0.40 2.36x þ 3.04x2 1.25 0.79x þ 1.65x2 1.65 0.39x þ 1.05x2 2.25 þ 0.25x þ 0.49x2 3.02 þ 0.97x þ 0.40x2

Remark QF QF a a a a a

Bowing parameter is obtained from V. R. D’Costa et al. (Phys. Rev. B 73, 125207 (2006))

6.2.2 Ternary Alloy (a) CSiGe As mentioned in Section 1.4.3, CxSiyGe1xy can be grown lattice-matched on Si substrate. The smaller C addition compensates the compressive strain in SixGe1x binary layers and thus relieves thickness limitations in SixGe1x growth. Furthermore, the major band offset in SixGe1x/Si heterojunction is in the CB, which, in connection with the VB offset in the SixGe1x/Si, has already been opened up a wide variety of new electronic and optical properties within the SixGe1x/Si heterojunction system. Amour et al. [38] have grown pseudomorphic CxSiyGe1xy/Si(100) layers by rapid thermal CVD and measured PL spectra at temperatures between 2 and 77 K. We show in Figure 6.11 the lowest gap energy EgL versus biaxial compressive strain for pseudomorphic SixGe1x (adopted

146

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.2

E Lg (eV)

1.1

pm - Si xGe 1-x z =0.24

1.0 z =0.38 0.9 pm - Cx Si y Ge 1-x-y

0.8

0

0.005

0.010 e bcs

0.015

0.020

Figure 6.11 Energies of the fundamental absorption edge EgL versus biaxial compressive strain ebcs for pseudomorphic (pm-) SixGe1x and pm-CxSiyGe1xy (z ¼ 1xy) at 77 K. The experimental data are taken from Amour et al. [38] (solid and open circles). The pm-SixGe1x line is taken from Van de Walle and Martin [39]. The ebcs ¼ 0 compositions are estimated to be x ¼ 0.05 (0.03) and y ¼ 0.57 (0.73) for z ¼ 0.38 (0.24)

from Van de Walle and Martin [39]) and Amour’s data. Adding C into SixGe1x and keeping the constant Ge content, the strain decreases and EgL increases, but the increase in EgL is much less than it would be if the strain was reduced simply by reducing the Ge content without adding C atoms. Amour et al. considered that for a given band gap, CxSiyGe1xy has less strain than does SixGe1x. The average slope of the CxSiyGe1xy data, DEgL /Debcs ¼ 6.1 eV/unit strain, corresponds to DEgL /Dx ¼ þ 21 meV/at%[C] [38]. Furthermore, by linearly extrapolating the CxSiyGe1xy data to zero ebcs, a significant band offset to Si for strain-free CxSiyGe1xy films is obtained. For z ¼ 1 x y ¼ 0.38, the band offset would be 0.19 eV. From Table 1.8, we can estimate the ebcs ¼ 0 compositions to be x ¼ 0.05 (0.03) and y ¼ 0.57 (0.73) for z ¼ 0.38 (0.24). Schmidt and Eberl [40] grew strained, exactly strain compensated and compressively strained CxSiyGe1xy layers on Si by MBE and measured their PL spectra at 8 K. In Figure 6.12 EgL has been plotted against Ge composition for exactly strain compensated, relaxed CxSiyGe1xy layers obtained by Schmidt and Eberl. Note that the EgL energies plotted in Figure 6.12 were obtained from the zero-phonon PL peaks by adding the indirect-exciton binding energy to coincide with the value of EgL ¼ 1.17 eVat 8 K for bulk Si [1]. These plots can be fitted by a linear decrease with DEgL /Dz ¼ 8.4 meV/at%[Ge], or equivalently, DEgL / Dx ¼ 68 meV/at%[C]. Schmidt and Eberl [40] also observed an initial increase in PL peak energies on the way from tensile strained CxSi1x as well as from compressively strained SixGe1x towards exactly strain compensated CxSiyGe1xy.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

147

1.17 1.16 r - Siy Ge1-x

E Lg (eV)

1.15 1.14 1.13 1.12

sc-Cx Siy Ge1-x-y

1.11

T =8 K

1.10 1.09 0

1

2

3

4 5 Ge (at%)

6

7

8

Figure 6.12 Energies of the fundamental absorption edge EgL versus Ge atomic composition for exactly strain compensated (sc-) CxSiyGe1xy layers at 8 K reported by Schmidt and Eberl [40]. The EgL energies were estimated from the zero-phonon PL peaks by adding the indirect-exciton binding energy to coincide with the band gap of EgL ¼ 1.17 eV at 8 K for bulk Si. For comparison, the relaxed (r-) SiyGe1y line is plotted against Ge atomic composition

The higher-lying CPs, such as E1 and E2, in CxSiyGe1xy/Si(100) films were studied using SE and ER [18,41,42]. The E1 gap increased and the E2 gap decreased as x increased for Si-rich CxSiyGe1xy alloy [41,42]. For Ge-rich CxSiyGe1xy alloy, C had no detectable influence on the higher-lying CPs [18]. (b) SiGeSn Single-phase SixGeySn1xy alloys with x 0.25 and y 0.64 were grown on Si(100) by CVD [43,44]. SE of selected samples yielded dielectric functions indicating a band structure consistent with highly crystalline semiconductors of diamond symmetry. Incorporation of Si into GexSn1x led to an additional reduction of E2, as expected based on the E2 values of Si and Ge [43].

6.2.3 Summary We have discussed the energy band gaps in some group-IV semiconductor alloys. Figure 6.13 summarizes the fundamental absorption gap Eg versus lattice constant a for some binary alloys. We find that all binary gaps, except for GexSn1x (0 x 0.88), are indirect. The GexSn1x alloy for 0.67 x 0.88 is a direct gap semiconductor, but becomes semimetallic for x 0.67. We can thus suppose that almost all ternary gaps, like CxSiyGe1xy, are indirect. CxSi1x is estimated to have an indirect gap at X (EgX ) over the whole composition range, while CxGe1x may have an indirect gap at L (EgL ) for 0 x 0.09 and at X for the rest. The band-gap energy of CxGe1x lattice-matched to 3C-SiC can be derived from Figure 6.13. The lattice constant a of 3C-SiC is 4.3596 A. The corresponding x and EgX for CxGe1x/3C-SiC are 0.62 and 3.7 eV, respectively. The fundamental absorption edge of 3C-SiC is 2.39 eV (EgX , Table 6.1). Because of its wide band-gap nature, C0.62Ge0.38 can be used as a new gate or a

148

PROPERTIES OF SEMICONDUCTOR ALLOYS 6 C 5

Eg (eV)

4 3 3C-SiC

2

Ge

1

Si

α -Sn

0 semimetallic -1 3.5

4.0

4.5

5.0

5.5

6.0

6.5

a (Å)

Figure 6.13 Lowest band-gap energy Eg versus cubic lattice constant a for some group-IV binary alloys at 300 K. The 3C-SiC data is plotted for comparison

barrier material for 3C-SiC FETs. It should be noted, however, that an interpolation scheme proposed by Soref [45] gives the nearly same EgX values between CxGe1x/3C-SiC alloy and 3C-SiC. The E1-gap bowing parameters c are determined to be 0.153 and 1.65 eV for SixGe1x and GexSn1x, respectively (Tables 6.4 and 6.5). In Figure 6.14 these values are plotted against the product DaABDXAB of the lattice constant (DaAB) and electronegativity differences (DXAB) between the elemental semiconductors A and B. The electronegativity values were taken from Phillips’s definition [46]. The bowing parameter c increases almost linearly with increasing product DaABDXAB (c in eV, DaABDXAB in AeV) c ¼ 9:93ðDaAB DXAB Þ

ð6:8Þ

4.0 3.5

E1

3.0

SiSn

c (eV)

2.5 2.0

GeSn

1.5 1.0 0.5 0

SiGe 0

0.1 ∆a ∆X AB

AB

0.2 (Å eV)

0.3

Figure 6.14 Bowing parameter c of the E1 gap versus product DaABDXAB of the lattice-constant and electronegativity differences between the endpoint elements A and B in the binary alloy AxB1x. The SiSn data (open circle) is taken from D’Costa et al. [44]. The solid line represents the calculated result using Equation (6.8)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

149

D’Costa et al. [44] obtained c 3.05 eV for SixSn1x from the SE analyses in the E1/(E1 þ D1) region of SixGeySn1xy. The open circle in Figure 6.14 represents the data of D’Costa et al. We can conclude that the c values in the Si–Ge–Sn alloy system follows a simple scaling behavior that can be expressed in terms of the electronegativity and lattice mismatches (Equation (6.8)). It should be noted, however, that Equation (6.8) estimates in considerably large bowing parameters c for C-related alloys, 20, 24 and 39 eV for CxSi1x, CxGe1x and CxSn1x, respectively. Further study is, therefore, needed to elucidate this unexpected point.

6.3 III–V SEMICONDUCTOR TERNARY ALLOY 6.3.1 (III, III)–N Alloy (a) c-AlGaN Due to their metastable nature, the growth of single-phase cubic nitride films of sufficient homogeneity and crystal quality is still difficult and, in general the crystal quality of the cubic III–N layers grown so far is inferior to that of the hexagonal nitrides. The E0 edge of cAlxGa1xN has been studied using SE [47–49]. These results are shown in Figure 6.15(a). We can see that the experimental data of Kasic et al. [49] gives larger E0 values than those obtained by Suzuki et al. [48]. As a result, the linear interpolation scheme explains Kasic’s data very well, as shown by the heavy solid line. The electronegativity and size mismatch

6 (a) c-AlxGa1-xN

(b) c-GaxIn1-xN

(c) c-AlxIn1-xN

5

E0, E gX (eV)

4 E gX 3

2

c=0 eV c=-1.000 eV E0

1

0 c-AlN

c-GaN

c-InN

c-AlN

x

Figure 6.15 Energies of the lowest direct E0 and indirect gaps EgX for (a) c-AlxGa1xN, (b) c-GaxIn1xN and (c) c-AlxIn1xN at 300 K. The experimental data in (a) are taken from Suzuki et al. [48] (solid circles) and Kasic et al. [49] (open circles) and in (b) from M€ullh€auser et al. [71] (open circle) and Goldhahn et al. [72] (solid circles). The theoretical curves are calculated from Table 6.6

150

PROPERTIES OF SEMICONDUCTOR ALLOYS

product scale also predicts a very small bowing parameter c 0.07 eV for c-AlxGa1xN (Equation (6.23)). No experimental data has been reported on the X- and L-valley gaps EgX and EgL for any binary nitrides or their alloys. All theoretical work, however, has suggested that in all III–N semiconductors the X-valley CB is located at a lower energy than the L-valley CB (i.e. EgX < EgL ) [50]. Thompson et al. [51] carried out SE measurements on c-AlN and concluded from the gradual onset of the absorption edge that c-AlN is an indirect gap semiconductor. The gap that they obtained is 5.34 eV (EgX ). It should be noted, however, that it is very difficult to determine an indirect absorption edge, which usually has very weak transition strength, using SE. Thus, optical absorption or transmission measurements are needed to directly determine whether c-AlN is a direct or an indirect gap semiconductor. The light solid line in Figure 6.15(a) shows the linear interpolation result of the theoretical EgX values for c-AlN and c-GaN [50]. The corresponding EgX and E0 versus x formulas are listed in Table 6.6. The heavy dashed line also represents the result of Equation (A.5) with c ¼ 1.000 eV. This value is recommended for wAlxGa1xN (c ¼ 1.00 eV, see Table 6.7). The E1 and E2 CPs in c-AlxGa1xN are also found to be blue- and red-shifted respectively, with increasing x for x 0.12, [49]. (b) w-AlGaN The experimental E0 versus x data for w-AlxGa1xN [52–55] are shown in Figure 6.16(a). The bowing parameter c of E0 varies widely from upward to deep downward bowing [56,57]. Lee et al. [58] noted that the early findings of an upward bowing have generally not been duplicated. Although there have been many reports of c for x < 0.4, very few data have been reported for

Table 6.6 Energies for some direct and indirect gaps in cubic (III, III)–N tenaries at 300 K. LF ¼ linear fit; LI ¼ linear interpolation; QF ¼ quadratic fit Ternary

Band gap

Expression (eV)

Remark

AlxGa1xN

E0 E0 EgX E0 EgX E0 EgX

3.231 þ 1.969x 3.231 þ 0.969x þ 1.000x2 4.20 þ 1.14x 0.56 þ 4.64x 3.00 þ 2.34x 0.560 þ 2.671x 3.0 þ 1.2x

LF (LI) QF LI LI LI LF (LI) LI

AlxIn1xN GaxIn1xN

Table 6.7 Energy for E0 in some wurtzite (III, III)–N tenaries at 300 K. QF ¼ quadratic Ternary

E0 (eV)

Remark

AlxGa1xN AlxIn1xN GaxIn1xN

3.42 þ 1.78x þ 1.00x2 0.70 þ 1.80x þ 3.70x2 0.700 þ 1.080x þ 1.640x2

QF QF QF

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

151

7 (a) w-AlxGa1-xN

(b) w-GaxIn1-xN

(c) w-AlxIn1-xN

6

E 0 (eV)

5 4 3 2 1 0 c-AlN

c-GaN

c-InN

c-AlN

x

Figure 6.16 Energies of the lowest direct gap E0 for (a) w-AlxGa1xN, (b) w-GaxIn1xN and (c) w-AlxIn1xN at 300 K. The experimental data in (a) are taken from Brunner et al. [52] (solid circles), Muth et al. [53] (open circles), Meyer et al. [54] (solid triangles) and Buchheim et al. [55] (open triangles). The experimental data in (b) and (c) are taken from Wu and Walukiewicz [65] (solid circles), Androulidaki et al. [66] (open circles) and Terashima et al. [67] (solid triangles, (c)). The open squares in (a)–(c) represent the endpoint binary data taken from Table 6.2. The solid lines have been calculated from the data in Table 6.7

x > 0.5 [54,57,59]. It can be seen that such higher x samples tend to give smaller E0 values, although the w-AlN (x ¼ 1.0) value is relatively large (E0 6.2 eV, Figure 6.16(a)). The apparent observation of the stronger bowing in the higher x region is actually an artifact resulting from defect- or impurity-related transitions at energies below the band gap [60]. The solid line in Figure 6.16(a) shows the calculated E0 curve using a recommended value of c ¼ 1.00 eV, as summarized in Table 6.7. This value is in good agreement with the results of Yun et al. [61]. Wethkamp et al. [59] also reported the x dependence of the higher-lying CPs at E1 7 eV and E2 8 eV, together with an unidentified peak at E? 13 eV. The temperature and pressure dependence of the band-gap energies has been measured for III–N binaries [50]. There have, however, been relatively few studies on the III–N alloys. Malikova et al. [62] measured the temperature dependence of the excitonic A, B and C peaks in w-Al0.05Ga0.95N in the 16–434 K range using contactless ER and analyzing the results with Varshni and Bose–Einstein expressions [1]. Brunner et al. [52] measured the absorption spectra of MBE-grown w-AlxGa1xN (0 x 1.0) from 7 K up to room temperature, from which a negligible x dependence of the Varshni coefficients a and b was observed. More recently, Nepal et al. [63] employed deep-UV PL to study the temperature and composition dependence of the band-gap energies of MOCVD-grown w-AlxGa1xN (0 x 1.0) in the range between 10 and 800 K. A quadratic dependence of the Varshni coefficients a and b with x was obtained, from which we can calculate the band-gap energy of w-AlxGa1xN with optional x and T.

152

PROPERTIES OF SEMICONDUCTOR ALLOYS

The pressure dependence of E0 in w-AlxGa1xN at 0 x 0.6 grown by MOCVD on (0001)-sapphire substrates has been investigated by Shan et al. [64] for pressures of up to 9 GPa. They reported dE0/dp to be 40 meV/GPa. (c) c-AlInN No detailed experimental data has been reported on the band-gap energies in c-AlxIn1xN. We, therefore, show in Figure 6.15(c) the linearly interpolated results of E0 and EgX using the experimental and theoretical endpoint data, respectively (Table 6.6). (d) w-AlInN The recent experimental studies which reported the E0 of InN to be appreciably below 1 eV compared to the long-accepted value of 2 eV, have initiated a continuing controversy concerning this fundamental quantity of the least studied III–N binary compound, InN. Also, obtaining high-quality Al-based semiconductors (AlN, AlP, AlAs, etc.) is very difficult as a consequence of its significantly higher contamination with residual impurities. Thus, the standard quadratic expression did not provide a reasonable fit to the compositional variation of E0 in w-AlxIn1xN [56]. The experimental E0 versus x data for w-AlxIn1xN is shown in Figure 6.16(c). The recent literature data are taken from Wu and Walukiewicz [65], Androulidaki et al. [66] and Terashima et al. [67]. These data suggest relatively large downward bowing. The solid line in Figure 6.16(c) shows the parabolic fit of these experimental data. The recommended bowing parameter is very large, c 3.70 eV, as listed in Table 6.7. Goldhahn et al. [68] measured the SE spectra of w-AlxIn1xN at 0 x 0.29 in the energy range up to 9.5 eV and determined the higher-lying CPs E1–E4, together with E0. They increased gradually with increasing x. The bowing parameters c determined for E1 and E2 are 1.8 and 2.7 eV, respectively. The pressure dependence of E0 in w-Al0.25In0.75N has been studied by Li et al. [69]. They also estimated the pressure coefficients for w-AlxIn1xN and expressed them as dE0/dp ¼ 25 þ 20x meV/GPa. (e) c-GaInN The E0 gap in c-InN grown on 3C-SiC(100) has been determined to be 0.56 eV by SE at 300 K [70]. The E0 versus x data for c-GaxIn1xN has also been determined using SE [71,72]. These data together with the linearly interpolated EgX values are shown in Figure 6.15(b). The experimental E0 values are in good agreement with the linearly interpolated E0 result given by the heavy solid line (Table 6.6). (f) w-GaInN The recent crystal growth of high-quality GaxIn1xN epilayers with small x has considerably broadened the composition range over which the bowing could be determined reliably. The E0 versus x data for w-GaxIn1xN are shown in Figure 6.16(b). The data are taken from Wu and Walukiewicz [65] and Androulidaki et al. [66]. A number of larger studies cast doubt on the small bowing parameter in w-GaxIn1xN [56]. For example, the experimental data of Parker et al. [73] implied a bowing of 3.42 eV (4.11 eV) for strained (relaxed) GaxIn1xN epilayers grown on (0001)-sapphire substrates with x < 0.25. However, recent studies of a broad

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

153

compositional range supported the findings of a smaller bowing of 1.4 eV [65,74]. Our recommended bowing parameter in Figure 6.16(b) is 1.640 eV (Table 6.7). Higher-lying CPs have been observed in w-GaxIn1xN using SE [75]. A total of five CPs (A, E1, E2, E3 and E4), together with E0, are observed in the spectral range of 0.5–10 eV. All these CPs showed a weak nonlinearity with x. The E0 gap of w-InN is reported to be 0.70 0.05 eVat 300 K [76]. The Varshni coefficients for w-InN are also reported to be a ¼ 0.41 meV/K and b ¼ 454 K [65]. An up-to-date compilation of various band parameters has been presented in Adachi [1] for group-IV elemental, III–V and II–VI binary semiconductors. By using an interpolation scheme, therefore, it is in principle, possible to estimate the band-gap energies for group-IV, III–V and II–VI semiconductor alloys at any temperature and also any pressure. The temperature dependence of E0 in w-GaxIn1xN has been determined for x ¼ 0.86 [77] and 0.92 [78]. The Varshni coefficients a ¼ 1.0 meV/K and b ¼ 1196 K for x ¼ 0.86 [77] are nearly the same as those for w-GaN (a 1.3 meV/K and b 1200 K) [1]. The pressure dependence of E0 in w-GaxIn1xN with 0.89 x 1.0 grown by MOCVD has been investigated for pressures of up to 9 GPa [78]. The pressure coefficients dE0/dp are 37.5 2.5 meV/GPa (T ¼ 10295 K). The pressure coefficients for samples at 0.5 x 1.0 have also been determined and found to be dE0/dp ¼ 30 5 meV/GPa [69].

6.3.2 (III, III)–P Alloy (a) AlGaP AlxGa1xP has an indirect gap over the whole composition range. Figure 6.17(a) shows the lowest indirect and direct gap energies EgID and E0 as a function of x for AlxGa1xP. The experimental EgX data were obtained from optical absorption measurements [79]. The optical absorption at 6 K measured by Onton et al. [80] provided an indirect gap bowing of c 0.18 eV. More recent CL data obtained at 14 K [81] support a small bowing of 0.13 eV for the lowest indirect gap EgX . However, Figure 6.17(a) shows that good agreement with the experimental data can be achieved by putting c ¼ 0 eV into Equation (A.5). The lowest and higher-lying CPs in AlxGa1xP have been investigated using ER in early studies and SE more recently. The experimental E0 data plotted in Figure 6.17(a) are taken from such studies (Rodrıguez and Armelles [82], Choi et al. [83], etc.). The linear interpolation scheme provides good agreement with the experimental E0 data, as shown by the solid line. The composition dependence of the higher-lying CPs is shown in Figure 6.17(b). The experimental ER and SE data can be satisfactorily fitted by the linear expression against alloy composition x [83]. The corresponding formulas are listed in Table 6.8. Note that the SO split-off energies D0 and D1 are observed to be negligibly small in the III–P semiconductors. From Figure 6.17(b), we can expect crossing ofE00 and E2 at x 0.5, which may be a unique characteristic of this alloy (cf. Figure 6.19). If we simply exchange an assignment of the CPs, namely E00 $ E2, in AlP [83], no such crossing occurs, as demonstrated by the dashed lines in Figure 6.17(b). Note that the E00 and E2 transitions occur at or near the G and X points in the BZ, respectively (Figure 6.1), and that identifying higher-lying CPs is a very difficult task. (b) AlInP AlxIn1xP can be lattice-matched to GaAs at x 0.53. Onton and Chicotka [84] grew bulk AlxIn1xP by a modified Bridgman method and measured the CL spectra at 300 K. The open

154

PROPERTIES OF SEMICONDUCTOR ALLOYS 4.0

6

E2

(a) 5

E0

E0 ' 4

E gL

E gD (eV)

E0,E gID (eV)

3.5

3.0

3

E0 2

E gX

2.5

E1

AlxGa1-xP

1

(b) 2.0 0

0.2

0.4

0.6

0.8

1.0

0 0

x

0.2

0.4

0.6

0.8

1.0

x

Figure 6.17 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxGa1xP at 300 K. The experimental data for E0 are taken from Rodrıguez and Armelles [82], Choi et al. [83], etc., and for EgX from Sonomura et al. [79]. (b) Energies of some CPs versus x for AlxGa1xP at 300 K. The solid lines in (a) and (b) show the calculated results sing the data in Table 6.8. The dashed lines were also obtained by exchanging the E00 $ E2 CP assignment in AlP

Table 6.8 Energies for some indirect and direct gaps in AlxGa1xP at 300 K. LF ¼ linear fit; LI ¼ linear interpolation Band gap

Expression (eV)

Remark

EgX EgL E0 E1 E0 0 E2

2.261 þ 0.219x 2.63 þ 0.94x 2.76 þ 1.15x 3.71 þ 0.59x 4.74 þ 0.40x 5.28 0.65x

LF LI LF LF LF LF

circles in Figure 6.18(a) show these results. A G–X crossing is found to occur at x 0.45. Bour et al. [85] also grew a series of AlxIn1xP on GaAs (100) by MOCVD and determined the E0 energies by ER. These results are also shown in Figure 6.18(a) by the solid circles. The quadratic fit of E0 gives a value of c 0.40 eV, as listed in Table 6.9. No experimental data relating to the higher-lying CPs in AlxIn1xP has been reported. We, therefore, show in Figure 8.18(b) the CP energies obtained from the linear interpolation scheme between the InP (x ¼ 0) and AlP (x ¼ 1.0) data in Adachi [1]. As in Figure 6.17(b) (AlxGa1xP), crossing of E00 and E2 occurs at x 0.4 in AlxIn1xP. This crossing can be removed by simply exchanging the assignment of the CPs, E00 $ E2 , in AlP [83], as demonstrated by the dashed lines in Figure 8.18(b). The electron-HH and electron-LH transition energies in strained AlxIn1xP layers grown on GaAs by MOCVD were investigated at 20 K using a PR technique [86]. The E0 versus x data

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

6

4.0

E2

(a)

5

3.0

E0 '

4

E gL

E gD (eV)

E0, E gID (eV)

3.5

2.5 E gX

3

E1

2

2.0

E0

E0

1.5 1.0

155

1

Al xIn 1-xP 0

0.2

0.4

0.6

0.8

1.0

0

0

(b) 0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.18 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxIn1xP at 300 K. The experimental data are taken from Onton and Chicotka [84] (open circles) and Bour et al. [85] (solid circles). (b) Energies of some CPs versus x for AlxIn1xP at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.9. The dashed lines are also obtained by exchanging the E00 $ E2 CP assignment in AlP Table 6.9 Energies for some direct and indirect gaps in AlxIn1xP at 300 K. QF ¼ quadratic fit; LI ¼ linear interpolation; LF ¼ linear fit Band gap

Expression (eV)

Remark

E0 EgL EgX E1 E00 E2

1.35 þ 2.16x þ 0.40x2 2.05 þ 1.52x 2.21 þ 0.27x 3.71 þ 1.13x 4.70 þ 0.44x 5.10 0.47x

QF LI LF LI LI LI

were also measured for relaxed AlxIn1xP at 20 K [86] and can be expressed as (in eV) E0 ðxÞ ¼ 1:418 þ 2:4x

ð6:9Þ

(c) GaInP GaxIn1xP exhibits some of the largest direct gaps among the non-nitride III–V semiconductors and can be grown lattice-matched to GaAs at x 0.52. This alloy is widely used as a material for various optoelectronic and electronic devices. The lowest direct gap E0 versus x for GaxIn1xP is shown graphically in Figure 6.19(a). The experimental data are taken from Onton et al. [87] (open circles) and Alibert et al. [88] (solid circles). The solid line represents the calculated E0 versus x curve by putting c ¼ 0.65 eV into Equation (A.5). This value is the same as that recommend in Vurgaftman et al. [89]. The G–X crossover is believed to occur at x 0.7 in GaxIn1xP. The indirect band-gap energies EgX for x 0.7 are plotted against x in Figure 6.19(a) by the open triangles. They are

156

PROPERTIES OF SEMICONDUCTOR ALLOYS 3.0

6

E2

(a) 5

E0 '

2.5

E gX

E gL

2.0

E gD (eV)

E0,E gID (eV)

4

0

0.2

0.4

0.6

0.8

E0+∆0

E0

1

Gax In1-x P 1.0

E1

3 2

E0

1.5

E1+∆1

1.0

0 0

(b) 0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.19 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaxIn1xP at 300 K. The experimental data for E0 are taken from Onton et al. [87] (open circles) and Alibert et al. [88] (solid circle) and for EgX from Alibert et al. [88], Lange et al. [90], etc. (open triangles). (b) Energies of some CPs versus x for GaxIn1xP at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.10

taken from Alibert et al. [88], Lange et al. [90], etc. The solid lines represent the calculated EgX and EgL curves using c ¼ 0.200 and 0.34 eV, respectively. Early theoretical and experimental bowing parameters are summarized by Bugajski et al. [91] and more recent values by Vurgaftman et al. [89]. These results vary widely: c ¼ 0.39–1.36, 0–0.40 and 0.23–0.86 eV for E0, EgX and EgL , respectively. Clearly, the c ¼ 1.03 eV value for EgL recommended by Vurgaftman et al. [89] is out of the reported range of 0.23–0.86 eV. If we assume here that c ¼ 0.34 eV for EgL, which is exactly the same as Hill’s value [92], the c ¼ 0.200 eV value for E0 is also the same as that recommended by Vurgaftman et al. [89] (c ¼ 0.20 eV). The expressions for such energy gaps are summarized in Table 6.10. Table 6.10 Energies for some direct and indirect gaps in GaxIn1xP at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

1.35 þ 0.76x þ 0.65x2 1.46 þ 0.73x þ 0.65x2 2.05 þ 0.24x þ 0.34x2 2.210 0.149x þ 0.200x2 3.17 0.32x þ 0.86x2 3.29 0.33x þ 0.86x2 4.70 þ 0.04x 5.10 þ 0.18x

a a b b c c LI LI

Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) Bowing parameter is obtained from R. Hill (J. Phys. C: Solid State Phys. 7, 516 (1974)) c Bowing parameter is obtained from C. Alibert et al. (Phys. Rev. B 6, 1301 (1972)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

157

The composition dependence of the higher-lying CPs for GaxIn1xP has been investigated using ER [88] and SE [93]. These studies observed remarkable bowing (c 0.9 eV) for the E1 and E1 þ D1 transitions. The GaxIn1xP samples used by Lee et al. [93] were epitaxially grown on GaAs and graded-GaInP/GaP substrates by various techniques, such as MOCVD, gassource MBE, LPE or HT-VPE. They mainly investigated the strain and disorder effects of the electrical and optical properties. The general behavior of the E1/(E1 þ D1) peak shifts was explained in terms of the biaxial strain and strain relaxation caused by lattice mismatch. The solid lines in Figure 6.19(b) show the results calculated from Table 6.10. Since the SO split-off energies D0 and D1 are mainly characterized by the nature of the anion atom, the common anion alloys like GaxIn1xP and ZnxCd1xTe have nearly the same D0 or D1 energies, irrespective of alloy composition x. Therefore, in such alloys the E0 þ D0 and E1 þ D1 gaps have nearly the same bowing parameters as the E0 and E1 gaps, respectively. The temperature dependence of the fundamental absorption edge of GaxIn1xP (x ¼ 0–1.0) has been investigated from 20 to 300 K by Ishitani et al. [94]. The same studies, but using samples lattice-matched to GaAs (x 0.5), have also been carried out using PzR [95] and SE [96]. The measured data were analyzed using some empirical expressions, such as Varshni and Bose–Einstein formulas. Onton and Chicotka [97] also undertook PL measurements on GaxIn1xP at 2 K and obtained the x-dependent E0 and EgX values given by (in eV) E0 ðxÞ ¼ 1:409 þ 0:695x þ 0:758x2

ð6:10Þ

EgX ðxÞ ¼ 2:321 þ 0:017x

ð6:11Þ

The pressure dependence of the fundamental absorption edge of GaxIn1xP has been determined by several authors [98,99]. The pressure coefficients dE0/dp and dEgX /dp reported by Hakki et al. [98] were 125 5 meV/GPa (x 0.5) and 11.5 1.5 meV/GPa (x ¼ 0–1.0), respectively. Go~ ni et al. [99] found from optical absorption studies that G–X crossing occurred at 5.0 GPa for x ¼ 0.36 and at 2.7 GPa for x ¼ 0.5 at 300 K. PL measurements were also carried out to investigate G–X crossing as a function of pressure for GaxIn1xP epilayers grown on GaAs(100) substrates [100,101].

6.3.3 (III, III)–As Alloy (a) AlGaAs AlxGa1xAs is known to be the most important and the most investigated III–V semiconductor alloy. Figure 6.20(a) shows the lowest direct and indirect gaps E0, EgL and EgX versus x for AlxGa1xAs. Theexperimentaldatafor E0 aretakenfromAubel etal. [102] and Aspnes etal.[103], for EgL from Saxena [104] and for EgX from Monemaret al. [105].The solid lines are calculated from the data in Table 6.11. The expression for E0 is determined from the SE analysis [103]. This expression reveals that the bowing parameter is x-dependent in the manner (in eV) shown below E0 ðxÞ ¼ ¼

1:430 þ 1:707x1:437x2 þ 1:310x3 1:430 þ 1:580x þ xð1xÞð0:1271:310xÞ

ð6:12Þ

Using Equation (6.12), we can obtain good agreement with the experimental results. It should be noted, however, that almost all AlxGa1xAs data have been explained by the quadratic expression with c ranging from 0.25 to þ 1.147 eV [106].

158

PROPERTIES OF SEMICONDUCTOR ALLOYS

6 3.0

(a)

2.5

E gX

2.0

E0 '

4

E gL E gD (eV)

E0, E gID (eV)

E2

5

E1+∆1 E1

3 E0+∆0

E0

2 E0

1.5

1

Alx Ga1-x As 1.0

0

0.2

0.4

0.6

0.8

1.0

x

0

0

(b) 0.2

0.4

0.6

0.8

1.0

x

Figure 6.20 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxGa1xAs at 300 K. The experimental data for E0 are taken from Aubel et al. [102] and Aspnes et al. [103] (open circles), for EgL from Saxena [104] (solid circles) and for EgX from Monemar et al. [105] (solid triangles). (b) Energies of some CPs versus x for AlxGa1xAs at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.11. The dashed line in (b) also represents the result calculated using Equation (6.13)

Many reports support the hypothesis that the c value for EgL is almost equal to zero. Lee et al. [107], however, reported a value of c ¼ 0.055 eV from PL measurements. The plots produced by Saxena [104] also suggested c ¼ 0 eV for EgL, independent of temperature [108]. As seen from Figure 6.20(a), GaAs is a direct gap semiconductor with G–L–X valley ordering, while AlAs is an indirect gap semiconductor with exactly the reverse ordering. The G–X crossover composition xc for AlxGa1xAs was determined at various temperatures [106] and found to be 0.4 at 300 K and 0.38 at low temperatures. The higher-lying CPs in AlxGa1xAs have been determined by many authors [106]. The bowing parameter of c 0.39 eV was reported for E1, while the E2 gap showed an almost liner variation with x. Such results are shown in Figure 6.20(b) (see also Table 6.11). Aspnes Table 6.11 Energies for some direct and indirect gaps in AlxGa1xAs at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

1.430 þ 1.707x 1.437x2 þ 1.310x3 1.72 þ 0.65x 1.760 þ 1.053x þ 0.407x2 1.910 þ 0.185x þ 0.055x2 2.890 þ 0.518x þ 0.392x2 3.130 þ 0.479x þ 0.391x2 4.52 þ 0.10x 5.13 0.26x

a LI b c b b LI LI

Bowing parameter is obtained from D. E. Aspnes et al. (J. Appl. Phys. 60, 754 (1986)) Bowing parameter is obtained from J. L. Aubel et al. (J. Appl. Phys. 58, 495 (1985)) c Bowing parameter is obtained from H. J. Lee et al. (Phys. Rev. B 21, 659 (1980)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

159

et al. [103] reported an expression analogous to Equation (6.12) for E1 (in eV) E1 ðxÞ ¼ 2:924 þ 0:965x þ xð1xÞð0:1570:935xÞ

ð6:13Þ

The dashed line in Figure 6.20(b) represents the calculated result of this expression. Traditionally, temperature variation of the band-gap energy Eg is expressed in terms of the Varshni formula [1] Eg ðTÞ ¼ Eg ð0Þ

aT 2 T þb

ð6:14Þ

where Eg(0) is the band-gap energy at 0 K, a is in electron volts per Kelvin and b is closely related to the Debye temperature of the material (in Kelvin). The E0-gap Varshni parameters E0(0), a and b for AlxGa1xAs are shown in Figure 6.21(a). The experimental data were 15

β (K)

2.5

(a)

(b)

2.0

12

1.5 11 10 9 8 7 6 5 4 350 300 250 200 150

dE0/dp (10-2eV/GPa)

α (eV/K)

E0(0) (eV)

3.0

9

6 AlxGa1-xAs

3

0

0.2

0.4

0.6 x

0.8

1.0

0 0

0.2

0.4

0.6

0.8

1

x

Figure 6.21 (a) Varshni parameters Eg(0), a and b versus x for E0 in AlxGa1xAs. The solid lines represent the liner least-squares fits summarized in Table 6.12. (b) Pressure coefficient dE0/dp versus x for AlxGa1xAs. The experimental data are taken from Adachi [106]. The solid line shows the calculated result using Equation (6.15)

gathered from various sources. The solid lines represent the linear least-squares fits summarized in Table 6.12. The Varshni parameters for EgL and EgX are also listed in Table 6.12. Introducing such parameters into Equation (6.14), we obtain the E0, EgL and EgX energies for optional alloy compositions (0 x 1.0) and T from 0 up to at least 400 K. The Varshni parameters for the higher-lying CPs were reported in Adachi [106]. There is some considerable variation in the absolute pressure coefficients of E0 and they are limited to x 0.5 [106]. However, the literature data in Figure 6.21(b) can probably be best summarized by (in 102 eV/GPa) dE0 ðxÞ ¼ 11:61:1x ð6:15Þ dp

160

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.12 Varshni parameters defined by Equation (6.14) for E0, EgL and EgX in AlxGa1xAs Band gap

Eg(0) (eV)

a (104 eV/K)

b (K)

E0a EgL b EgX b

1.513 þ 1.380x 1.775 þ 0.792x 1.988 þ 0.207x þ 0.055x2

5.8 þ 3.6x 6.1 4.6–1.0x

206 þ 123x 204 204

Obtained from Figure 6.21 S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties. World Scientific, Singapore, 1994 a b

The EgL and EgX data showed no clear x-dependent pressure coefficients that can be approximated as dEgL =dp 5:5 102 eV=GPa and dEgX =dp 1:5 102 eV=GPa [106]. The pressure coefficients of E1 and E1 þ D1 were approximated as (78) 102 eV/ GPa [106]. (b) AlInAs AlxIn1xAs can be grown lattice-matched to InP at x 0.48 and serve as a barrier layer in the important Ga0.47In0.53As/Al0.48Ga0.52As/InP heterostructure system. Wakefield et al. [109] undertook CL measurements on AlxIn1xAs/InP(100) at x 0.5 and obtained a value of c ¼ 0.74 eV for E0. More recently, Chou et al. [110] determined c 0 eV from PR in the limited composition range 0.43 x 0.58. The experimental data of Chou et al. (solid circles) are shown in Figure 6.22(a). The E0 energy for Al0.48In0.52As/InP was reported to be 1.439 0.005 eV at 300 K [111]. The open circle in Figure 6.22(a) shows this data. From these data, we obtain a value of c 0.72 eV, in good agreement with the earlier work of Wakefield et al. [109].

6

3.5

(a)

3.0

E0 '

4

2.0

E gD (eV)

E0,E gID (eV)

2.5 E gX

1.5 E gL

1.0

0.2

E1 E0+∆0

2

0.4

0.6 x

0.8

E0

1

Alx In1-x As 0

E1+∆1 3

E0

0.5 0

E2

5

(b) 1.0

0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.22 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxIn1xAs at 300 K. The experimental data are taken from Chou et al. [110] (solid circles) and Oertel et al. [111] (open circle). (b) Energies of some CPs versus x for AlxIn1xAs at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.13

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

161

The linear interpolation scheme, used to estimate the L- and X-valley minima, also implies G–X crossover occurring at x 0.63 in Figure 6.22(a). The higher-lying CPs in AlxIn1xAs have been studied using SE [82] and normal-incidence reflectivity [112]. These studies determined the E1-gap c value to be 0.86 and 0.38 eV, respectively. Avalue of c ¼ 0.39 eV was also determined for E1 þ D1 [112]. The recommended band-gap expressions for AlxIn1xAs are summarized in Table 6.13. Table 6.13 Energies for some direct and indirect gaps in AlxIn1xAs at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

0.359 þ 1.931x þ 0.720x2 0.726 þ 1.774x þ 0.720x2 1.07 þ 1.30x 1.37 þ 0.78x 2.50 þ 0.92x þ 0.38x2 2.78 þ 0.83x þ 0.39x2 4.44 þ 0.18x 4.70 þ 0.17x

a b LI LI c c LI LI

Obtained from Figure 6.22 Postulated bowing parameter equal to that for E0 c Bowing parameter is obtained from A. Convertino et al. (J. Vac. Sci. Technol. B 20, 248 (2002))

a b

(c) GaInAs GaxIn1xAs remains a direct gap material over the whole composition range. We show in Figure 6.23(a) the lowest direct and indirect gaps E0, EgL and EgX versus x for GaxIn1xAs. The E0 versus x data are taken from Nahory et al. [113] (open circles) and Kim et al. [114] (solid circles). Ga0.47In0.53As/InP has an energy E0 ¼ 0.728 0.002 eV at 300 K [115]. The open triangle in Figure 6.22(a) shows this value. From these data points, we obtain a value of c 0.58 eV for E0, slightly larger than that recommended by Vurgaftman et al. [89] (c ¼ 0.477 eV). Singh [116] reviewed the E0 gap in lattice-matched and strained Ga0.47aIn0.53 þ aAs grown on InP(100). He obtained the following expression for unstrained samples with small a at 300 K (in eV) E0 ðaÞ ¼ 0:751:05a þ 0:45a2

ð6:16Þ

with zero HH–LH splitting, while for strained samples (in eV) E0 ðaÞ ¼ 0:750:63a þ 0:45a2

ð6:17Þ

with HH–LH splitting of 0.42a eV. There is no reliable experimental technique to determine the L- and X-valley gaps EgL and EgX in GaxIn1xAs. The c values in Table 6.14 are assumed to have a composite value in the range compiled by Vurgaftman et al. [89]. The dashed lines in Figure 6.22(a) represent the EgL and EgX values calculated using Vurgaftman’s recommended c values.

162

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.0

6

(a)

(b)

E2

5 E gX

E0 '

4 1.0

E gD (eV)

E0, E gID (eV)

1.5

E gL

E0

E1+∆1

3

E1

2

E0+∆0

0.5 1

Gax In1-x As 0 0

0.2

0.4

0.6

0.8

E0 1.0

x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.23 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaxIn1xAs at 300 K. (b) Energies of some CPs versus x for GaxIn1xAs at 300 K. The experimental data in (a) and (b) are taken from Nahory et al. [113] (open circles), Kim et al. [114] (solid circles) and Gaskill [115] (open triangle). The solid lines in (a) and (b) show the calculated results using the data in Table 6.14. The dashed lines in (a) are calculated using c ¼ 0.33 and 1.4 eV for EgL and EgX , respectively

The higher-lying CPs in GaxIn1xAs have been determined using SE [114]. These results are shown in Figure 6.23(b). The samples were grown on InP(100) at a thickness of 1 mm, which exceeds the critical thicknesses of strain relaxation. Thus, the data presented in Figure 6.23 represent those for bulk materials. Andreani et al. [117] used PR and SE to investigate the optical response and energy-band structure of a series of strained and relaxed GaxIn1xAs (x > 0.85) films on GaAs(100) substrates. They observed that the energy shifts in E1 and E1 þ D1 due to built-in strain were in good agreement with those calculated from standard DP theory. The solid lines in Figure 6.23(b) were obtained by the analysis of Kim’s data [114] or using the linear interpolation scheme. These results are summarized in Table 6.14. Table 6.14 Energies for some direct and indirect gaps in GaxIn1xAs at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

0.359 þ 0.491x þ 0.580x2 0.726 þ 0.454x þ 0.580x2 1.07 þ 0.15x þ 0.50x2 1.37 0.16x þ 0.70x2 2.50 0.16x þ 0.55x2 2.78 þ 0.03x þ 0.32x2 4.44 þ 0.08x 4.70 þ 0.43x

a b c c d d d LI

Obtained from Figure 6.23 Postulated bowing parameter equal to that for E0 c Estimated from list by I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) d Estimated from data by T. Y. Kim et al. (Phys. Rev. B 68, 115323 (2003)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

163

2.0

E0(0) (eV)

1.5

GaxIn1-xAs

1.0 (a)

0.5 0

α (eV/K)

6 5 4 (b)

3 2 500 β (K)

400

(c)

300 200 100 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.24 Varshni parameters Eg(0), a and b versus x for E0 in GaxIn1xAs. The solid lines represent the liner least-squares fits of Equation (6.18)

The Varshni parameters E0(0), a and b for E0 in GaxIn1xAs are plotted in Figure 6.24. The experimental data have been gathered from various sources (e.g. Hang et al. [118]). The solid lines show the liner least-squares fits given by E0 ð0ÞðxÞ ¼ 0:359 þ 1:154x eV

ð6:18aÞ

aðxÞ ¼ ð3:3 þ 2:5xÞ 104 eV=K

ð6:18bÞ

bðxÞ ¼ 21711x K

ð6:18cÞ

No detailed pressure dependence of the band-gap energies in GaxIn1xAs has been reported. It should be noted, however, that the pressure dependence for GaAs and InAs can be given by dE0/dp ¼ 107 and 114 meV/GPa [1], respectively. Thus, we suggest the value of dE0/dp for GaxIn1xAs to be 110 meV/GPa, independent of x.

6.3.4 (III, III)–Sb Alloy (a) AlGaSb The bowing parameter c for E0 in AlxGa1xSb was determined using various techniques, such as PL, optical absorption and ER [119–121]. The reported c values varied widely from 1.18

164

PROPERTIES OF SEMICONDUCTOR ALLOYS

to þ 0.69 eV [89]. Alibert et al. [119] obtained c ¼ 0.47 and 0.48 eV at room temperature and low temperatures, respectively, and made a detailed comparison between these and previous results. More recently, Bignazzi et al. [120] obtained a better fit to the optical absorption data assuming a linear band-gap variation at low x. These results were confirmed by Bellani et al. [121] from TR measurements at T ¼ 90–300 K. Consequently, a cubic expression was proposed for E0 in AlxGa1xSb E0 ðxÞ ¼ 0:723 þ 1:547x þ ð0:0441:220xÞxð1xÞ ¼ 0:723 þ 1:591x1:264x2 þ 1:220x3

ð6:19Þ

The calculated result of this expression is shown in Figure 6.25(a), together with the experimental data [119,121]. The experimental data in the higher x region in Figure 6.25(a) suggest that the X-valley gap EgX has no strong composition dependence. The experimental G–L crossover composition also suggests that the bowing parameter may be negligibly small for EgL [89]. 5

2.5 Alx Ga1-x Sb

E2 4

2.0

E0 '

1.5

E gD (eV)

E0,E gID (eV)

E gL E gX

E0

1.0

3

E1 2

1

0.5

(a) 0

0

0.2

0.4

0.6 x

0.8

E1+∆1

E0+∆0 E0 (b)

1.0

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.25 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxGa1xSb at 300 K. The experimental data are taken from Anderson et al. (see Alibert et al. [119]) (open circles) and Bellani et al. [121] (solid circles). The solid line (E0) shows the calculated result using Equation (6.19). (b) Energies of some CPs versus x for AlxGa1xSb at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.15

The higher-lying CPs in AlxGa1xSb have been studied using modulation spectroscopy, such as PzR and ER [119,122] and SE [123,124]. The bowing parameters obtained from these studies are in the range 0.28–0.63 eV. Since the data of Choi et al. were limited to 0 x 0.39 [124], they were fitted using a linear expression. The recommended band-gap expressions for AlxGa1xSb are summarized in Table 6.15. The linear temperature coefficient dE0/dT was reported to be 4 104 eV/K for 0 x 1.0 [121] and x 0.4 [122]. The linear temperature coefficient dEgX =dT was also reported to be (3.1 0.2) 104 eV/K for x > 0.52 [119]. The Varshni parameters E0(0), a and b have been determined for x ¼ 0.12 and 0.19 [125]. However, pressure studies have not been carried out on AlxGa1xSb.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

165

Table 6.15 Energies for some direct and indirect gaps in AlxGa1xSb at 300 K. LI ¼ linear interpolation; LF ¼ linear fit Band gap

Expression (eV)

Remark

E0 EgL EgX E0 þ D0 E1 E1 þ D1 E00 E2

0.723 þ 1.591x 1.264x2 þ 1.220x3 0.760 þ 1.451x 1.050 þ 0.565x 1.50 þ 1.04x þ 0.40x2 2.05 þ 0.49x þ 0.30x2 2.50 þ 0.43x þ 0.30x2 3.56 þ 0.20x 4.14 þ 0.09x

a LI LF b c c LI LI

Bowing parameter is obtained from V. Bellani et al. (Phys. Rev. B 59, 12272 (1999)) Estimated from E0 data c Estimated from various data a b

(b) AlInSb Very limited data are available for AlxIn1xSb [126–128]. Isomura et al. [126] recorded the ER spectra for AlxIn1xSb at 0 x 1.0. They determined the E0, E0 þ D0, E1 and E1 þ D1 energies versus x at 300 K and their results are shown in Figure 6.26, together with those for EgL, EgX , E00 and E2 estimated from the linear interpolation scheme. The corresponding band-gap expressions are listed in Table 6.16. The data in Figure 6.26(a) suggest that AlxIn1xSb is a direct gap semiconductor at x 0.7.

2.5

5 Alx In1-x Sb

E2

2.0

4

E0 '

1.5

E gD (eV)

E0, E gID (eV)

E gX E gL

1.0

3

2

E1+∆1 E1

E0 0.5

1

E0

(a) 0 0

0.2

0.4

0.6 x

0.8

E0+∆0

1.0

0 0

(b)

0.2 0.4 0.6 0.8 1.0 x

Figure 6.26 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxIn1xSb at 300 K. The experimental data are taken from Isomura et al. [126] (solid circles). (b) Energies of some CPs versus x for AlxIn1xSb at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.16

166

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.16 Energies for some direct and indirect gaps in AlxIn1xSb at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.17 þ 1.67x þ 0.930 þ 1.281x 1.04 þ 1.16x þ 1.630 0.015x 1.80 þ 0.70x þ 2.30 þ 0.72x þ 3.26 þ 0.50x 3.90 þ 0.33x

a

Remark 0.43x2 0.74x2 0.34x2 0.21x2

a LI a LI a a LI LI

Bowing parameter is estimated from data in S. Isomura et al. (Phys. Status Solidi B 65, 213 (1974))

The bowing parameters obtained from Isomura et al. [126] are 0.34 and 0.21 eV for E1 and E1 þ D1, respectively, while those obtained by Yaozhou et al. [127] are about a factor of 2 larger and are 0.752 and 0.723 eV for E1 and E1 þ D1, respectively. The fundamental absorption edges in AlxIn1xSb layers (0 x 0.25) grown on GaAs substrates were studied by Dai et al. [128] using transmission spectroscopy from cryogenic to room temperature. A linear change of E0 with lattice constant a (or x) was obtained. (c) GaInSb GaxIn1xSb remains a direct gap semiconductor over 0 x 1.0. The bowing parameters c for E0 previously reported are c ¼ 0.413 0.43 eV for bulk samples [129–131] and 0.35 eV for epilayers [132]. A more recent study of a GaxIn1xSb/GaSb(100) epilayer reports c ¼ 0.406 0.009 eV [133], which is in much better agreement with the bulk results. The solid circles in Figure 6.27(a) show the PzR results obtained by Auvergne et al. [130], which give an E0 bowing of 0.415 eV. The considerable uncertainty for the indirect gaps in GaSb (x ¼ 0) and especially InSb (x ¼ 1.0) translates into a poor understanding of the L- and X-valley gap bowing. The c values of 0.40 and 0.33 eV for EgL and EgX in Table 6.17 are taken from Vurgaftman et al. [89]. The higher-lying CPs, E1, E1 þ D1, E00 and E2, in GaxIn1xSb have been studied using ER [129] and SE [134]. The bowing parameters determined from these studies are in reasonable agreement and are shown in Table 6.17 and Figure 6.27(b). The linear temperature coefficient dE0/dT obtained from PzR measurements [130] can be written as (2.75 1.05x) 104 eV/K. Therefore, the linear interpolation scheme can be safely used to obtain the temperature-dependent and may also be used to estimate the pressuredependent band-gap energies in GaxIn1xSb. The necessary binary data are compiled from Adachi [1].

6.3.5 Dilute-nitride III–(V, V) Alloy (a) General Considerations Dilute-nitride III–V alloys, such as GaNxAs1x and GaInNxAs1x, represent a new class of highly mismatched material systems, which have recently attracted great attention [135]. The ‘dilute’ nitrides now mean that a small N fraction of the order of a few percent can be added to a

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS 2.0

5

(a)

(b)

GaxIn1-xSb

E2

4

1.5 E gX 1.0 E gL 0.5

E gD (eV)

E0,E gID (eV)

167

E0

E0 '

3

E1+∆1 2

E1 E0+∆0

1

E0 0

0

0.2 0.4 0.6 0.8 1.0

0

0

0.2 0.4 0.6 0.8 1.0

x

x

Figure 6.27 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaxIn1xSb at 300 K. The experimental data are taken from Auvergne et al. [130] (solid circles). (b) Energies of some CPs versus x for GaxIn1xSb at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.17

conventional non-nitride semiconductor, such as GaAs or GaInAs. Due to large differences in the lattice constant and ionicity between the host binary and N-related binary (Table 6.18), the dilute nitrides exhibit many unusual and fascinating physical properties. Among them the most prominent feature is the giant bowing in the band-gap energy. It is known that a single bowing parameter is inadequate even if the goal is only to describe the band-gap energy for a relatively wide range of compositions. For example, the bowing parameter c for E0 in GaNxAs1x reached 40 eV for a very low N incorporation (x 0.1 at%), and strongly decreased with increasing N fraction [136]. Because of this, we do not recommend that the type of bowing parameter c be used to describe the dilute nitrides [56].

Table 6.17 Energies for some direct and indirect gaps in GaxIn1xSb at 300 K Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.170 þ 0.135x þ 0.415x2 0.93 0.57x þ 0.40x2 1.040 þ 0.045x þ 0.415x2 1.63 0.91x þ 0.33x2 1.80 0.13x þ 0.38x2 2.30 0.08x þ 0.28x2 3.26 þ 0.30x 3.90 þ 0.24x2

a b c b d d d d

Bowing parameter is obtained from D. Auvergne et al. (J. Phys. Chem. Solids 35, 133 (1974)) Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) c Postulated bowing parameter equal to that for E0 d Bowing parameter is obtained from S. M. Vishnubhatla et al. (Can. J. Phys. 47, 1661 (1969)) a b

168

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.18 Lattice mismatch Da/a and Phillips ionicity difference Dfi for some III–(V, V) and (III, III)–V ternaries. Note that III–(N, V) ternaries exhibit ‘strongly perturbed’ characteristics Alloya

|Da|/a (%)

|Dfi|

Alloy b

|Da|/a (%)

|Dfi|

Al(N, P) Al(N, As) Al(N, Sb) Ga(N, P) Ga(N, As) Ga(N, Sb) In(N, P) In(N, As) In(N, Sb)

19.8 22.6 28.6 17.1 20.0 34.9 15.0 21.5 23.0

0.142 0.175 0.199 0.173 0.190 0.239 0.157 0.221 0.257

(Al, Ga)P (Al, Ga)As (Al, Ga)Sb (Ga, In)P (Ga, In)As (Ga, In)Sb Ga(P, As) Ga(P, Sb) Ga(As, Sb) In(P, As) In(P, Sb) In(As, Sb)

0.2 0.1 0.6 7.1 6.7 5.9 3.6 10.6 7.3 3.1 9.4 6.5

0.020 0.036 0.011 0.094 0.047 0.060 0.017 0.066 0.049 0.064 0.100 0.036

a b

Strongly perturbed alloy Weakly perturbed alloy

The unexpected properties of various dilute nitrides are incompatible with standard models (e.g. VCA) describing semiconductor alloys. Many proposals have been developed, which can be summarized in the three main models: (1) impurity band formation [137,138], (2) BAC model [139,140] and (3) a polymorphous alloy model [141,142]. The subtle distinction between the three models lies in the evolution of the localized N states and the host CB states in the alloys [143]. The impurity band model argues that the CB minimum evolves from interacting N-related impurity states (isolated N centers, N pairs and clusters) and requires no participation of higher-lying host CB states [137,138]. The BAC model includes a mutual repulsion between the N level and G-valley CB state [139,140]. N-induced perturbed host states in the third model, on the other hand, covers all host CB states that are affected by the perturbation induced by nitrogen [141,142]. There is no perfect model to fully explain the unique properties of the dilute-nitride alloys; the dispute still continues [144–146]. It has, however, been well established that the electronic energy-band consequence of such materials can be simply parameterized in terms of the BAC model [56]. If the effect of the VB is completely neglected, the N states lead to a characteristic splitting of the CB into two subbands E ðkÞ ¼

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 ðEC ðkÞ þ EN Þ ðEC ðkÞEN Þ2 þ 4V 2 x 2

ð6:20Þ

where EC(k) is the CB dispersion of the unperturbed non-nitride semiconductor, EN is the position of the N isoelectronic impurity level in that semiconductor, V is the interaction potential between the two subbands and x is the N fraction. The CB structure for GaNxAs1x obtained from Equation (6.20) with EC(0) ¼ 1.43 eV (E0), EN ¼ 1.65 eV and V ¼ 2.70 eV is shown in Figure 6.28. Any temperature dependence arises from the shift of the CB dispersion EC(0) in Equation (6.20), which is assumed to follow the Varshni, Bose–Einstein or other expression [1],

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

169

2.4

2.1

Energy (eV)

E+ 1.8

EC

EN

1.5 E0 (GaAs)

E-

GaNxAs1-x

1.2 k

Figure 6.28 CB dispersion relationships for diluted-nitride GaNxAs1x calculated from Equation (6.20). For comparison, the unperturbed GaAs CB (EC) and the position of the N level (EN) are shown

whereas EN is assumed to be independent of T. In dilute-nitride alloys the DP interaction should be treated carefully, with a view to the much weaker shift of EN with pressure. The pressure or strain dependence of the E transitions should be determined by substituting the appropriate DPs of the host semiconductor to obtain EC(k) and then deriving E(k) from Equation (6.20) or an even more detailed formalism. The effect of N incorporation on the electron effective mass is more subtle. In general, the smaller the E0 gap, the smaller the CB effective mass meG [1]. However, measurements on all diluted nitrides have shown an increase in the electron effective mass meG. The band-anticrossing-induced enhancement of the DOS electron effective mass can be calculated from the dispersion relationship E(k) in Equation (6.20) by [145] " # 2 k V x mGe ðkF Þ ¼ h2 ¼ mGe 1 þ ð6:21Þ dE ðkÞ=dkk¼kF ðEN E ðkF ÞÞ2 where meG represents the host material value at k ¼ 0. The Fermi wavevector kF and Fermi energy EF ¼ E(kF) can be determined from the free-electron concentration. Note that Equation (6.21) suggests an increase in mGe with increasing x. Since N incorporation mainly affects the CB states, the band anticrossing effect should not alter the VB structure, and as a result, the hole effective masses, appreciably. Similarly, since the band-gap bowing occurs mainly as a result of the lowering of the CB edge, a large CB offset and a small discontinuity in the VB edge should be expected. If we consider unstrained dilute nitride, the VB offset should be safely set equal to that of the host semiconductor material. The electron mobility is expected to be lower in dilute nitrides due to strong alloy or impurity scattering and the enhanced electron effective mass. It is well known that the G-valley electron mobility decreases with increasing meG [1]. Since reduced mobility of both electrons and holes has been observed, alloy or impurity scattering is likely the dominant effect governing carrier mobility, especially electron mobility.

170

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b) GaNP Nitrogen is known to form a series of isoelectronic traps in GaP. The oscillator strength of the interband transitions in N-doped GaP can be strongly enhanced by increasing N concentrations up to the alloy limit, due to N-induced admixing of the G component to the lowest CB states of the alloy leading to the crossover from an indirect gap in GaP to a direct gap in GaNxP1x with a surprisingly low N concentration of around 0.5 at% [140,147–149]. Figure 6.29(a) shows the N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxP1x. The experimental data are taken from Buyanova et al. [150]. The horizontal arrows indicate the positions of E0, EgX and EgL in the host semiconductor GaP. The solid lines represent the results calculated according to Equation (6.20) using EC(k ¼ 0) ¼ 2.76 eV (E0), EN ¼ 2.25 eV and V ¼ 3.10 eV (Table 6.19). Note that EN ¼ 2.25 eV is slightly smaller than the well-known isoelectronic NN states at 2.18 eV in GaP [151]. The determined N level EN ¼ 2.25 eV is placed nearly at the X-point CB minimum EgX ¼ 2.261 eV (Table 6.1). The EN and V values reported by Buyanova et al. [150] are, respectively, 2.25 and 2.76 eV, while those recommended by Vurgaftman and Meyer [56] are 2.18 eV (EN) and 3.05 eV (V) respectively. 3.4

2.4 (a) GaNxP1-x

3.2

2.8 E (eV)

2.2 E+

3.0

1.6 E gX

2.0 1.8

E0 E gL

2.6

1.8

2.4 E gX

2.0

X

E-

0.8

1.6 1

2 3 x (at%)

4

5

E0

0.4

0

1

2 3 x (at%)

E-

0.2

(b) GaNxAs1-x

0.6 0

E gL

0.8 0.6

1.0

4

E+

Eg

1.0

1.2 E-

1.8

1.2

E0

1.4

2.2

1.4

E+ E gL

1.6

(c) GaNxSb1-x

5

0 0

1

2 3 x (at%)

4

5

Figure 6.29 (a) N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxP1x at 300 K. The experimental data are taken from Buyanova et al. [150]. (b) N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxAs1x at 300 K. The experimental data for E are taken from Wu et al. [160] and for E þ from Gil [161]. (c) N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxSb1x at 300 K. The experimental data are taken from Jefferson et al. [178]. The solid lines in (a)–(c) represent the BAC results of Equation (6.20) using the model parameters in Table 6.19. The horizontal arrows indicate the positions of the E0, EgX and EgL gaps in the host semiconductor GaP, GaAs or GaSb

The CPs in GaNxP1x have been studied by Leibiger et al. [152] using SE at energies between 1 and 8.5 eV. They observed the G-point CPs E0 and E00 and L-direction CPs E1 and E10, together with two additional CPs labeled E21 and E22 , which cannot be assigned unambiguously. A strong blueshift of E0 and E1 was observed with increasing N incorporation, in contrast to the well-known downshift of the CB edge. The E00, E10, E21 and E22 CPs did not significantly shift with increasing N concentration.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

171

Table 6.19 BAC parameters EN and V calculated from Equation (6.20) for some dilute-nitride III–V ternaries and quaternaries at 300 K. Ternary

EN (eV)

V (eV)

Remark

GaNxP1x GaNxAs1x GaNxSb1x InNxP1x InNxAs1x InNxSb1x GaxIn1xNyAs1y

2.25 1.65 0.78 2.00 1.45 0.74 1.44 þ 0.21x

3.10 2.70 2.60 3.50 2.00 2.10 2.7 4.2x þ 3.5x2

a b c d e f g

Flit-determined from Figure 6.29 W. Shan et al., Phys. Rev. Lett. 82, 1221 (1999) c P. H. Jefferson et al., Appl. Phys. Lett. 89, 111921 (2006) d K. M. Yu et al., J. Appl. Phys. 90, 2227 (2001) e Flit-determined from Figure 6.31 f Modeled result of kp calculation shown in Figure 6.31 g I. Vurgaftman and J. R. Meyer, J. Appl. Phys. 94, 3675 (2003) a b

The CB edge E and G-point CB minimum E þ versus temperature have been measured by Ruko et al. [149] and Buyanova et al. [150]. The pressure dependence of E has also been reported [140,153]. These studies ruled out the previous assertion that the G–X transitions dominate the band gap in GaNxP1x at low N concentrations [154]. (c) GaNAs Among the dilute-nitride III–Valloys, GaNxAs1x was first grown epitaxially and represented a relatively new material system with unusual physical properties and potential technological importance [155]. A huge bowing of 18 eV was found in GaNxAs1x, which is equivalent for small N concentrations to a linear model with that slope [156]. Few attempts have been made to quantify the strong composition dependence of the band-gap energy, assuming a compositiondependent bowing parameter [157], a two-level BAC model [139,140], in the form of an arbitrary function [136,158] or a DEg/xa (a ¼ 2/3) scaling rule [159]. Figure 6.29(b) plots the fundamental gaps E and E þ as a function of x for GaNxAs1x. The experimental data for E are taken from Wu et al. [160] and for E þ from Gil [161]. The BAC results of Equation (6.20) are indicated by the solid lines. They are calculated using EN ¼ 1.65 eV and V ¼ 2.70 eV (Table 6.19) and follow the parameterization of Shan et al. [139]. The increase in E þ with increasing x is nearly equal to the band-gap reduction (DEg), indicative of a N-induced level repulsion. The CP energies versus x in GaNxAs1x were determined using SE [162–167] and PR [167,168]. These studies reported the blueshifted E1 and E1 þ D1 peaks, together with an uncommonly strong disorder-induced broadening, with increasing x. As in GaNxP1x, no clear peak shift was observed for E00 and E2 CPs [164,165,168]. A strong dependence of D0 on composition has also not been observed [169]. The linear temperature coefficient dE0/dT is 4.4 104 eV/K for GaAs at T 300 K [1]. A significant reduction in the temperature coefficient of the fundamental absorption edge has been reported for GaNxAs1x [170–173]; typically dE/dT ¼ 3 104 eV/K for x 3

172

PROPERTIES OF SEMICONDUCTOR ALLOYS

at% [170,172]. Similarly, the linear pressure coefficient dE0/dp for GaAs is 1.2 101 eV/ GPa [1], while a value for dE/dp of 7 102 eV/GPa was observed for GaNxAs1x with x ¼ 0.1 at% at T ¼ 33 130 K [174]. Such weak external perturbation dependence of E in GaNxAs1x is in good agreement with the BAC model [145]. The GaNxAs1x alloy at high N concentration is an attractive material for extending the wavelength range of GaN-based optoelectronic devices toward the red/IR region. The fundamental absorption edges of such As-poor (N-rich) alloys have been studied by several authors [156,175,176]. These results are shown in Figure 6.30 together with those obtained in the As-rich region [160]. The solid line shows the quadratic fit given by (E in eV) E ¼ 1:4311:7x þ 13:5x2

ð6:22Þ

3.5 3.0

c-GaNxAs1-x

2.5 2.0 E- (eV)

1.5

Quadratic fit BAC model

1.0 0.5 0 -0.5 -1.0 -1.5

semimetallic 0

0.2

0.4

x

0.6

0.8

1.0

Figure 6.30 Lowest absorption edge E versus x for c-GaNxAs1x at 300 K. The experimental data are taken from Wu et al. [160] (open circles), Kimura et al. [175] (solid triangles) and Wu et al. [176] (open triangles). The solid line represents the quadratic least-squares fit of Equation (6.22), while the dashed line shows the BAC result of Equation (6.19) using the model parameters in Table 6.19

This fit provides huge bowing of c ¼ 13.5 eV and thus results in a semimetallic overlap of the CB and VB at the intermediate compositions 0.15 x 0.73. It should be noted, however, that the 0.4 eV band-gap reduction observed with x 3 at% in Figure 6.30 is similar to that measured with an N fraction of x 15 at% [177]. No upper limit for the N concentrations for which the BAC model remains valid, has been identified so far [56]. (d) GaNSb There has been only one experimental report on the structural and optoelectronic properties of GaNxSb1x by MBE [178]. The GaNxSb1x layers (0.002 x 0.01) were grown on GaAs substrates. The band-gap energies were determined from FTIR measurements. The band-gap reduction DEg was solely due to the substitution of dilute amounts of highly electronegative N for Sb, and was greater than that observed in GaNxAs1x with the same N concentration. The results obtained by Jefferson et al. are shown in Figure 6.29(c) [178]. The solid lines show the fits of these data with Equation (6.20). The parameters determined using the BAC model are listed in Table 6.19.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

173

(e) InNP Several experiments have been carried out on InNxP1x [179,180]. Bi and Tu [179] incorporated N atoms into InP by gas-source MBE using N radicals and observed the linear reduction DEg with increasing N concentration. The value of DEg is about 0.15 eV at x ¼ 1 at%. More recently, Yu et al. [180] obtained dilute-nitride InNxP1x films by N þ ion implantation into InP with N doses up to 4.8 at%. The InNxP1x layers were thermally stable up to an annealing temperature of 850 C. The data of Yu et al. are shown in Figure 6.31(a) [180]. These data are nearly the same as those obtained by Bi and Tu [179]. The solid lines represent the BAC model results calculated using Equation (6.20) and the numeric parameters in Table 6.19. (f) InNAs There have been several experimental studies on the band-gap reduction in InNxAs1x [181– 184]. All these studies showed that the band gap was reduced with increasing x, as shown in Figure 6.31(b). The solid lines in Figure 6.31(b) represent the results calculated using

2.6 2.4

E gX

E+

2.2 E gL

E (eV)

2.0 1.8 1.6 1.4

E0

1.2 E-

1.0 0.8 0.6 0

(a) InNxP1-x 1

2 3 x (at%)

4

2.0 1.4 1.8 (b) InNxAs1-x 1.2 1.6 1.0 E+ X 1.4 0.8 Eg 1.2 0.6 E gL 1.0 0.4 0.8 0.2 0.6 0 E0 0.4 -0.2 0.2 -0.4 E0 -0.6 semimetallic -0.2 -0.8 5 0 1 2 3 4 5 0 x (at%)

E gL

E+

(c) InNxSb1-x E0

Esemimetallic

2

4 6 x (at%)

8

10

Figure 6.31 (a) N concentration dependence of the CB edge E and G-point CB minimum E þ in InNxP1x at 300 K [180]. (b) N concentration dependence of the CB edge E and G-point CB minimum E þ in InNxAs1x at 300 K [181–184]. (c) N concentration dependence of the CB edge E and G-point CB minimum E þ in InNxSb1x at 300 K. The solid lines in (a) and (b) and dashed lines in (c) represent the BAC results of Equation (6.20) using the model parameters in Table 6.19, while the solid lines in (c) show kp calculation made by Veal et al. [187]. The horizontal arrows indicate the positions of the E0, EgX and EgL gaps in the host semiconductor InP, InAs or InSb

Equation (6.20) with EN ¼ 1.45 eV and V ¼ 2.00 eV (Table 6.19). The effective N level EN ¼ 1.45 eV is nearly equal to those reported by Shih et al. [182] and Veal et al. [184] (1.48 eV). The interaction potential V ¼ 2.00 eV is slightly larger than those in Shih et al. [182] (1.68 eV), Kuroda et al. [183] (1.86 eV) and Veal et al. [184] (1.77 eV). The higher-lying CPs E1 and E1 þ D1 in InNxAs1x were studied using SE [185]. They were blue-shifted at a rate of 20–25 meV/at%[N].

174

PROPERTIES OF SEMICONDUCTOR ALLOYS

(g) InNSb Murdin et al. [186] measured the electron effective mass near the band anticrossing point by CR in InNxSb1x with the absorption edge near 15 mm. The observed results directly demonstrate band anticrossing and quantitatively confirm an increase in the effective mass predicted by a tight binding calculation for low N concentration (x < 1 at%). More recently, Veal et al. [187] formed a thin InNxSb1x layer by low-energy N implantation on InSb and found from XPS that N occupies 6 at% of the anion sublattice sites. Using HREELS, they also observed the absence of a depletion layer, indicating that the Fermi level is located below the VB maximum. Consequently, the CB minimum is located below the VB maximum, meaning that a negative band-gap material has been formed. These results are consistent with the kp calculation that predicts a semimetallic band structure, as shown by the solid lines in Figure 6.31(c) [187]. The dashed lines in Figure 6.31(c) show the parameterization fits of the kp results (solid lines) using Equation (6.20). The resulting parameters are found to be EN ¼ 0.74 eV and V ¼ 2.10 eV (Table 6.19).

Table 6.20 Energies for some indirect and direct gaps in some Al–(V, V) tenaries at 300 K Ternary

Band gap

Expression (eV)

Remark

AlPxAs1x

EgX EgL E0 EgX EgL E0 EgX EgL E0

2.15 0.07x þ 0.40x2 2.37 þ 0.82x þ 0.38x2 3.01 þ 0.77x þ 0.13x2 1.615 þ 0.588x þ 0.277x2 2.211 þ 0.603x þ 0.756x2 2.27 0.49x þ 2.13x2 1.615 þ 0.285x þ 0.250x2 2.211 0.315x þ 0.474x2 2.27 0.45x þ 1.19x2

a a b a a b a a b

AlPxSb1x

AlAsxSb1x

Bowing parameter is obtained from a theoretical study by A.-B. Chen and A. Sher (Semiconductor Alloys. Plenum, New York, 1995) b Bowing parameter is estimated from Equation (6.23) a

6.3.6 Al–(V, V) Alloy The minimum gaps in the Al-based III–V ternaries AlPxAs1x, AlPxSb1x and AlAsxSb1x are an indirect band gaps throughout their whole composition range with the CB minimum located in the vicinity of the X point, as shown in Figure 6.32. The various curves have been calculated from the data in Table 6.20. The bowing parameters c for E0 are estimated from the product of the lattice constant and electronegativity differences (Equation (6.23)). The bowing parameters c for EgL and EgX are obtained from the theoretical calculations by Chen and Sher [188]. Very few studies have been carried out on the determination of the energy-band structures for the Al–(V, V) ternaries. Saadallah et al. [189] have studied the photothermal properties of an MBE-grown AlAs0.08Sb0.92/GaSb layer. From the absorption spectrum they obtained, we can

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

175

4

(c) AlAsx Sb1-x

E0,E gID (eV)

3

2

E0 EgX EgL

1

(a) AlPx As1-x 0 AlP

(b) AlAsx Sb1-x AlAs

AlSb

AlP

x

Figure 6.32 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlPxAs1x, (b) AlAsxSb1x and (c) AlPxSb1x at 300 K. The solid circle in (b) is estimated from an optical absorption spectrum by Saadallah et al. [189]. The various curves in (a)–(c) represent the calculated results using the data in Table 6.20

estimate an absorption edge at 800 nm (1.55 eV). The solid circle in Figure 6.32(b) represents this data.

6.3.7 Ga–(V, V) Alloy (a) GaPAs GaPxAs1x remains a direct gap material in the composition range 0 x 0.48 at room temperature. Above x 0.48, the alloy becomes indirect because the X-valley minimum crosses below the G-valley minimum. The bowing parameter for E0 reported previously lies within a relatively narrow range c ¼ 0.174–0.21 eV [89]. The lowest direct and indirect gaps for GaPxAs1x as determined by ER [190] and PL measurements [191], respectively, are shown in Figure 6.33(a). The c ¼ 0.24 eV value for EgX recommended by Vurgaftman et al. [89] lies approximately in the middle of the previously reported range of 0.20–0.28 eV. The same authors also recommended a value of c ¼ 0.16 eV for EgL. The higher-lying CPs, such as E1, E1 þ D1, E00, E00 þ D00, E2 and E2 þ d, in GaPxAs1x have been determined by ER [190], reflectivity [192] and SE [193]. The kinks in the slope of the composition dependence of E1 and E1 þ D1 are found at x 0.5 [190,192]. A recent SE study does not confirm such an anomaly, but observes some alloy disorder effects, i.e. a large positive bowing for E0 and a large reduction in the E1/(E1 þ D1) strengths at x 0.5 [193]. The large bowing reported is c ¼ 0.54 eV, which is larger by more than a factor of 2 than the commonly accepted values (0.20–0.28 eV). This large bowing effect has not been verified and relies on only two data points with intermediates at x ¼ 0.4 and 0.7. All CPs higher than E1/(E1 þ D1) showed an almost linear increase with x [190,192,193], as shown in Figure 6.33(b). The recommended band-gap expressions are listed in Table 6.21. The temperature effects on the fundamental absorption edge especially near the E0 EgX crossover region in GaPxAs1x were studied using PL [191,194] and optical absorption [195]. As the temperature was increased to above 77 K, marked changes in PL were observed for both

176

PROPERTIES OF SEMICONDUCTOR ALLOYS 3.0

6

E2

(a) 5

E0 '

4

EgL EgX

2.0

E gD (eV)

E0,E gID (eV)

2.5

E0

E1+∆1 E1

3 2

E0+∆0

E0

1.5

GaPx As1-x 1.0 0

0.2 0.4 0.6 0.8 1.0 x

1 0 0

(b) 0.2 0.4 0.6 0.8 1.0 x

Figure 6.33 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaPxAs1x at 300 K. The experimental data are taken for E0 from Thompson et al. [190] (open circles) and for EgX from Craford et al. [191] (solid circles). (b) Energies of some CPs versus x for GaPxAs1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.21

N-doped and N-free alloys [191]. In both cases the higher-energy or near-band-edge process dominated the emission as the temperature was increased. Zero-phonon as well as phononassisted transitions were identified in the intrinsic absorption edge [195]. (b) GaPSb There are very few reports relating to GaPxSb1x in the literature [196,197]. The intrinsic absorption edge in GaPxSb1x as a function of x obtained by PL measurements is shown in

Table 6.21 Energies for some direct and indirect gaps in GaPxAs1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

1.43 þ 1.14x þ 0.19x2 1.72 þ 0.75x þ 0.16x2 1.76 þ 0.90x þ 0.18x2 1.910 þ 0.111x þ 0.240x2 2.89 þ 0.82x 3.13 þ 0.69x 4.52 þ 0.22x 5.13 þ 0.15x2

a a b a c c c c

Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) Bowing parameter is fit-determined from experimental data reported by A. G. Thomson et al. (Phys. Rev. 146, 601 (1966)) c Bowing parameter (c ¼ 0 eV) is obtained from A. G. Thompson et al. (Phys. Rev. 146, 601 (1966)) and K. J. Kim et al. (J. Appl. Phys. 84, 3696 (1998)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

177

Figure 6.34(a) [196,197]. The solid lines represent the E0, EgX and EgL versus x data obtained by putting c ¼ 2.7 eV into Equation (A.5). This bowing parameter is taken from Vurgaftman et al. [89]. Although the experimental data scatter largely, the curves of the calculated results explain the experimental data very well. From Figure 6.34(a), we can expect the E0 EgX crossover to occur at x 0.4. 3.0 2.5

6

(b)

GaPx Sb1-x

5

E2

E0 EgL

1.5

E0 '

4 E gD (eV)

E0, E gID (eV)

2.0

EgX

E1+∆1

3

E1

1.0

2

0.5

1

E0+∆0 E0

(a) 0 0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.34 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaPxSb1x at 300 K. The experimental data are taken from Jou et al. [196] and Loualiche et al. [197] (solid circles). (b) Energies of some CPs versus x for GaPxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.22

There have been no reports published concerning the higher-lying CPs in GaPxSb1x. We, therefore, assume the bowing parameters for E1 and E1 þ D1 to be a half of that for E0 and those for E00 and E2 to be a quarter of that for E0. Such trends can be found in some III–V ternary alloys (see e.g. GaAsxSb1x in Table 6.23). The solid lines in Figure 6.34(b) show the calculated results using the data in Table 6.22. Table 6.22 Energies for some direct and indirect gaps in GaPxSb1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL EgX E0 þ D0 E1 E1 þ D1 E00 E2

0.72 0.66x þ 2.70x2 0.76 0.83x þ 2.70x2 1.050 1.489x þ 2.700x2 1.50 1.36x þ 2.70x2 2.05 þ 0.31x þ 1.35x2 2.50 0.03x þ 1.35x2 3.56 þ 0.50x þ 0.68x2 4.14 þ 0.46x þ 0.68x2

a a a b c c d d

Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) Postulated bowing parameter equal to that for E0 c Bowing parameter is assumed to be a half of that for E0 (c ¼ 1.35 eV) d Bowing parameter is assumed to be a quarter of that for E0 (c ¼ 0.68 eV) a b

178

PROPERTIES OF SEMICONDUCTOR ALLOYS

(c) GaAsSb GaAsxSb1x remains a direct gap material over the whole composition range, as shown in Figure 6.35(a). The E0-gap bowing parameter has been determined using various techniques [89]. The experimental data plotted in Figure 6.35(a) were obtained from PL results by Nahory et al. [198] (solid circles) and from optical absorption measurements by Yano et al. [199] (open circles) and McGlinn et al. [200] (solid triangles). The quadratic fit of these data provides c ¼ 1.25 eV for E0. This value is slightly smaller than that recommended by Vurgaftman et al. [89] (c ¼ 1.43 eV). No experimental data are available for the c values of EgX and EgL . In Figure 6.35(a), the x-dependent EgX and EgL curves are calculated by introducing c ¼ 1.20 eV into Equation (A.5). These bowing parameters are recommended by Vurgaftman et al. [89]. 2.0

6

(a)

(b) 5

E2 EgX

1.0

EgL

E0 '

4 E gD (eV)

E0, E gID (eV)

1.5

E0

3

E1+∆1 E1

2

E0+∆0

0.5 1

GaAsx Sb1-x 0

0

0.2

0.4

E0 0.6

x

0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.35 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaAsxSb1x at 300 K. The experimental data are taken from Nahory et al. [198] (solid circles), Yano et al. [199] (open circles) and McGlinn et al. [200] (solid triangles). (b) Energies of some CPs versus x for GaAsxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.23

The higher-lying CPs have been investigated on MBE-grown GaAsxSb1x (0.56 x 1.0) on GaAs(100) substrates using PR [201] and those (0.35 x 0.78) grown on InP(100) substrates by MOCVD using SE [202]. Serries et al. [203] determined strained and relaxed E1/ (E1 þ D1) energies before and after correction for strain effects. The sample thickness used by Ferrini et al. [201] was in the range 0.6–1 mm for complete strain release at each mole fraction. The results obtained by these authors [201,203], together with those for E0 and E0 þ D0 (Table 6.23) are shown in Figure 6.35(b). The temperature dependence of E0 in GaAsxSb1x has been studied by several authors [203– 205]. Lukic-Zrnic et al. [204] obtained the Varshni parameters a and b, which describe not only their own data well, but also the previous data of Merkel et al. [203]. More recently, Chouaib et al. [205] obtained the Varshni parameters a¼(4.0 0.1) 104 ((3.9 0.1) 104) eV/K and b ¼ 143 18 (140 14) K for unintentionally doped (Si-doped) GaAsxSb1x/InP. These values are in reasonable agreement with those obtained by Lukic-Zrnic et al. [204]. Note that GaAsxSb1x can be grown lattice-matched to InP at x 0.5.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

179

Table 6.23 Energies for some direct and indirect gaps in GaAsxSb1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL EgX E0 þ D0 E1 E1 þ D1 E00 E2

0.72 0.54x þ 1.25x2 0.76 0.24x þ 1.20x2 1.05 0.34x þ 1.20x2 1.50 0.99x þ 1.25x2 2.05 þ 0.29x þ 0.55x2 2.50 þ 0.04x þ 0.59x2 3.56 þ 0.64x þ 0.32x2 4.14 þ 0.80x þ 0.19x2

a b b c d d e e

Flit-determined from Figure 6.35 Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) c Postulated bowing parameter equal to that for E0 d Bowing parameter is obtained from D. Serries et al. (J. Appl. Phys. 87, 8522 (2000)) e Bowing parameter is obtained from R. Ferrini et al. (J. Appl. Phys. 86, 4706 (1999)) a b

6.3.8 In–(V, V) Alloy (a) InPAs Due to the high vapor pressure of As and P elements, growth of InPxAs1x from the melt has received very little attention. Antypas and Yep [206] prepared InPxAs1x (0.735 x 1.0) by LPE and undertook PL measurements. Nicholas et al. [207] also grew InPxAs1x layers (0 x 1.0) by CVD and obtained their optical absorption spectra. More recently, Wada et al. [208] carried out both PL and absorption measurements on InPxAs1x layers (0.33 x 1.0) grown by MOCVD on InP(100) substrates. The E0 values for InPxAs1x obtained by these authors have been plotted in Figure 6.36(a). From these data, the bowing parameter c ¼ 0.145 eV for E0 can be obtained. Note, however, that the most recent data produced by Bui et al. [209] using PR, showed clear upward bowing of c ¼ 0.22 eV. Figure 6.36(a) also shows the composition dependence of EgX and EgL calculated from Equation (A.5) with the same c value as that for E0 (0.145 eV). ER measurements were carried out on InPxAs1x by Vishnubhatla et al. [129] and Thompson et al. [210]. Choi et al. [211] also used SE to investigate the band structure of InPxAs1x films on InP(100). The composition dependence of the higher-lying CPs, such as E1, E1 þ D1, E00 and E2 CPs, was determined from such investigations. Figure 6.36(b) shows the results of Vishnubhatla et al. [129]. Table 6.24 summarizes the numeric expressions. The temperature variation of E0 in InPxAs1x has been studied by Wada et al. [208]. The linear temperature coefficient dE0/dT for InP and InAs was reported to be 3.3 104 and 4.2 104 eV/K, respectively [1]. The InPxAs1x value obtained by Wada et al. is approximately 3 104 eV/K and is independent of x. (b) InPSb InPxSb1x may be an alternative material to Al-based semiconductor alloys, which commonly suffer from carbon and oxygen impurities. However, the predicted miscibility gap of this alloy

180

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.5

6

InPx As1-x

5

2.0

E0 '

4

1.5 E gD (eV)

E0,E gID (eV)

E gX

E2

E gL 1.0

E0 0.5

3

E1+∆1 E1

2 1

E0+∆0 E0

(a) 0 0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

x

0.4

0.6

(b) 0.8

1.0

x

Figure 6.36 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for InPxAs1x at 300 K. The experimental data are taken from Antypas and Yep [206] (solid circles), Nicholas et al. [207] (open circles) and Wada et al. [208] (solid triangles). (b) Energies of some CPs versus x for InPxAs1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.24

could limit its usefulness in device applications. Reihlen et al. [212] succeeded in growing InPxSb1x epilayers on InP, InAs and InSb by MOCVD and examined their optical properties. Duncan et al. [213] also grew an InPxSb1x/InP epilayer and obtained E0 ¼ 0.6 eVat 300 K from PL measurements. These results are shown in Figure 6.37(a). The least-squares fit of these data gives a bowing parameter of c ¼ 1.60 eV. This value is slightly smaller than c ¼ 1.9 0.1 eV obtained at 10 K by Jou et al. [196]. The solid lines in Figure 6.37(a) show the composition dependence of EgX and EgL and have been obtained by putting the same c values for E0 (1.60 eV) into Equation (A.5) since to date no alternative reliable data have been published.

Table 6.24 Energies for some direct and indirect gaps in InPxAs1x at 300 K Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

0.359 þ 0.846x þ 0.145x2 0.726 þ 0.589x þ 0.145x2 1.070 þ 0.835x þ 0.145x2 1.370 þ 0.695x þ 0.145x2 2.50 þ 0.42x þ 0.25x2 2.78 þ 0.26x þ 0.25x2 4.44 þ 0.24x þ 0.02x2 4.70 þ 0.37x þ 0.03x2

a b b b c c c c

Flit-determined from Figure 6.36 Postulated bowing parameter equal to that for E0 c Bowing parameter is obtained from S. S. Vishnubhatla et al. (Can. J. Phys. 47, 1661 (1969))

a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS 6

3.0

5 4

2.0 E gD (eV)

E0,E gID (eV)

(b)

InPx Sb1-x

2.5

EgX

1.5

E gL

1.0

3

E2 E0 ' E1+∆1 E1

2

E0

0.5

1

E0+∆0

(a) 0

181

0

0.2

0.4

0.6

0.8

E0 1.0

0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.37 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for InPxSb1x at 300 K. The experimental data are taken from Reihlen et al. [212] (solid circles) and Duncan et al. [213] (open circle). (b) Energies of some CPs versus x for InPxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.25

Since there have been no published reports relating to the higher-lying CPs in InPxSb1x, let us, therefore, assume the bowing parameters for E1 and E1 þ D1 to be a half of that for E0 and those for E00 and E2 to be a quarter of that for E0 (see Section 6.3.7(b)). The solid lines in Figure 6.37(b) represent the calculated results using such bowing parameters. The recommended band-gap expressions are summarized in Table 6.25. (c) InAsSb InSb has the smallest band gap among the III–V binary semiconductors (E0 ¼ 0.17 eV at 300 K). The InAsxSb1x alloy has the lowest band gap among all III–V semiconductors, with values as small as 0.1 eV at room temperature. The bowing parameter c for E0 previously Table 6.25 Energies for some direct and indirect gaps in InPxSb1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.17 0.42x þ 1.60x2 0.93 0.48x þ 1.60x2 1.04 1.18x þ 1.60x2 1.63 1.02x þ 1.60x2 1.80 þ 0.57x þ 0.80x2 2.30 þ 0.19x þ 0.80x2 3.26 þ 1.04x þ 0.40x2 3.90 þ 0.80x þ 0.40x2

a b b b c c d d

Flit-determined from Figure 6.37 Postulated bowing parameter equal to that for E0 c Bowing parameter is assumed to be a half of that for E0 (c ¼ 0.80 eV) d Bowing parameter is assumed to be a quarter of that for E0 (c ¼ 0.40 eV) a b

182

PROPERTIES OF SEMICONDUCTOR ALLOYS

reported for InAsxSb1x is 0.6 eV [89]. The values of E0 as a function of x for InAsxSb1x have been plotted in Figure 6.38(a). The experimental data have been obtained from Woolley and Warner [214], Stringfellow and Greene [215] and Dobbelaere et al. [216]. The least-squares fit of these data gives c ¼ 0.600 eV. The composition dependence of EgX and EgL obtained from Equation (A.5) using the same bowing parameter as that for E0 (c ¼ 0.60 eV) have also been plotted in Figure 6.38(a). 2.0

6 InAsx Sb1-x

(a)

(b) 5

EgX

EgL

1.0

E2

4 E gD (eV)

E0, E gID (eV)

1.5

3 2

0.5

E0 ' E1+∆1 E1

1

E0

E0+∆0 E0

0 0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.38 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for InAsxSb1x at 300 K. The experimental data are taken from Woolley and Warner [214] (open circles), Stringfellow and Greene [215] (open triangles) and Dobbelaere et al. [216] (solid circles). (b) Energies of some CPs versus x for InAsxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.26

SE was used to investigate the higher-lying CPs in InAsxSb1x [217]. The x-dependent E1, E1 þ D1 and E2 CPs were determined from this study. These results, together with those for E0 and E0 þ D0 CPs, are shown in Figure 6.38(b) and summarized in Table 6.26. Table 6.26 Energies for some direct and indirect gaps in InAsxSb1x at 300 K. LI ¼ linear interpolation. Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.170 0.411x þ 0.600x2 0.93 0.46x þ 0.60x2 1.04 0.914x þ 0.600x2 1.63 0.86x þ 0.60x2 1.8 þ 0.7x 2.30 þ 0.48x 3.26 þ 1.18x 3.9 þ 0.8x

a b b b c c LI e

Flit-determined from Figure 6.38 Postulated bowing parameter equal to that for E0 c Bowing parameter (c ¼ 0 eV) is obtained from H. Y. Deng and N. Dai (Phys. Rev. B 73, 113102 (2006))

a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

183

The Varshni parameters for E0 in InAs (InSb) are reported to be a ¼ 3.07 104 eV/K (2.7 104 eV/K) and b ¼ 191 K (106 K) [1]. The Varshni parameters for InAsxSb1x have also been determined by a number of authors, although the alloy composition was limited to a narrow region (see e.g. [218–222]). These data give the Varshni parameters of a 2.4 104 eV/K and b 180 K both of which are nearly independent of x, although the alloy composition was in the limited range x 0.06 or x 0.799. Only the data of Bansal et al. [220] gave the extremely large values of a ¼ 7.1 104 eV/K and b ¼ 675 K for x ¼ 0.05.

6.3.9 Summary This section has concentrated on reviewing the lowest direct and indirect gaps, together with some higher-lying CPs in III–V ternary alloys. These energy gaps have an approximately quadratic dependence on the mole fraction of one endpoint material x. The main emphasis is thus on the nonlinear or bowing parameter c. The lowest direct (E0) and indirect gaps (EgX ) versus composition x for some cubic III–V ternary alloys are shown in Figure 6.39. The degree of bowing varies quite considerably depending on the band gap in question. The large, positive bowing effect obtained in the VCA is largely a volume effect [4]. An impressive plot of a large parabola composed of the individual E0 versus x plots is shown in Figure 6.39 (AlAs–GaAs– –GaSb–AlSb). 5

E0, E gID (eV)

4

UV (He-Cd)

3

Blue (He-Cd) Green (Ar) Red (He-Ne)

2 E gX

IR (Nd3+:YAG)

1 E0

0 AlAs

GaAs

InAs

InSb

GaSb

AlSb

AlAs

AlP

GaP

InP

InN

GaN

AlN

x

Figure 6.39 Lowest direct E0 and indirect gaps EgX versus composition x for some cubic IIIV semiconductor ternary alloys at 300 K. The experimental data are shown by the open circles

Table 6.27 summarizes the bowing parameters c for E0, EgX and EgL in some (III, III)–V and III–(V, V) ternary alloys. The degree of bowing does not appear to be directly related to the binary energy steps. Figure 6.40 shows these parameters plotted against the product DaabDXab of the lattice constant and electronegativity differences between the endpoint binaries a and b. The electronegativity differences were obtained from Phillips’ data [46]. The solid line in Figure 6.40 represents the least-squares fit given by (c in eV, DaabDXab in AeV) c ¼ 9:62ðDaab DXab Þ

ð6:23Þ

Note that the proportionality factor 9.62 A1 in Equation (6.23) is slightly smaller than that 1 (9.93 A ) obtained in Equation (6.8). The c values for the Al–(V, V) ternary alloys shown in Table 6.20 are calculated from Equation (6.23).

184

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.27 Bowing parameters c for E0, EgX and EgL in some (III, III)–V and III–(V, V) ternaries (in eV) Ternary

E0

EgX

EgL

Ternary

E0

EgX

EgL

(Al, Ga)P (Al, In)P (Ga, In)P (Al, Ga)As (Al, In)As (Ga, In)As (Al, Ga)Sb (Al, In)Sb (Ga, In)Sb

0 0.40 0.65 0.127b 0.72 0.58 0.044b 0.43 0.415

0 0 0.200 0.055 0 0.70 0 0 0.33

0 0 0.34 0 0 0.50 0 0 0.40

Al(P, As) Al(P, Sb) Al(As, Sb) Ga(P, As) Ga(P, Sb) Ga(As, Sb) In(P, As) In(P, Sb) In(As, Sb)

0.13a 2.13a 1.19a 0.19 2.70 1.25 0.145 1.60 0.60

0.40 0.277 0.250 0.240 2.700 1.20 0.145 1.60 0.60

0.38 0.756 0.474 0.16 2.70 1.20 0.145 1.60 0.60

a b

Estimated from Equation (6.23) In the limit x ! 0 (see e.g. Equation (6.12))

3.0 2.5

GPS

c (eV)

2.0 IPS

1.5 GAS 1.0 GIP GIA

0.5 GPA 0

AlIA IAS AlIP

GIS AlIS

IPA 0

0.05

0.10

0.15

0.20

0.25

∆aAB∆XAB (ÅeV)

Figure 6.40 Bowing parameter c of the G-valley gap E0 versus product DaabDXab of the lattice-constant and electronegativity differences between the endpoint binary materials a and b in some IIIV semiconductor ternary alloys. The solid line represents the calculated result using Equation (6.23). G ¼ Ga; I ¼ In; A ¼ As; S ¼ Sb

6.4 III–V SEMICONDUCTOR QUATERNARY ALLOY 6.4.1 Dilute-nitride Quaternary Alloy (a) AlGaNAs The energy gaps in dilute-nitride AlxGa1xNyAs1y have been investigated by Shan et al. [180]. The energy positions of E and E þ can be explained by assuming an anticrossing interaction between states at the G minimum and located N state EN whose energy depends on x in the

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

185

following manner EN(x) ¼ 1.65 þ 0.61x eV. The E þ transitions lie above the G-valley CB minimum even in the indirect gap region of the AlxGa1xAs matrix. The results indicate that the N-induced interactions between the extended G, L and X CB states do not play a significant role in the modification of the CB structure of dilute-nitride III–V alloys. (b) GaInNP Some studies on GaxIn1xNyP1y have been carried out using PL [223,224] and PR [225,226]. All these studies suggested that N incorporation reduces the fundamental absorption edge of GaxIn1xP. The BAC parameters are EN ¼ 2.1 0.1 eV and V ¼ 1.7 0.2 eV for x ¼ 0.44–0.49 [224] and EN ¼ 2.040 eVand V ¼ 1.449 0.170 eV for x ¼ 0.46 [226]. A somewhat weaker temperature dependence of the band-gap energy was reported by Buyanova et al. [224], but Lin and Hwang [226] were unable to confirm such a weak temperature dependence. (c) GaInNAs Vurgaftman and Meyer [56] reviewed the results of studies on GaxIn1xNyAs1y. The addition of N narrows the band gap for lower In concentrations, while at the same time providing tensile strain compensation. Samples with very low In compositions in the order of 10 at% showed no significant difference from GaNxAs1x apart from the expected GaxIn1xAs gap decrease including bowing [56,89]. However, for samples with larger In contents grown on GaAs and InP, an alternative parameterization with the BAC model was proposed [227]. The interaction potentials V recommended for GaNxAs1x and InNxAs1x are 2.70 and 2.00 eV, respectively (Table 6.19). Pan et al. [228] took EN to be independent of the In concentration and used V ¼ 2.5 eV for GaxIn1xNyAs1y with x ¼ 0.7–0.9. Choulis et al. [229] made the same assumption regarding EN, but the interaction potential was considerably lower (V ¼ 1.675 eV). A similar value (V ¼ 1.7 eV) was independently proposed by Polimeni et al. [230] for x ¼ 0.24–0.41. On the other hand, Sun et al. [231] used V ¼ 2.8 3.0 eV to explain PL and PLE spectra in GaxIn1xNyAs1y/GaAs QWs (x ¼ 27.2 at%). Serries et al. [232] also obtained the V values for high In-containing GaxIn1xNyAs1y/InP films and showed the QWs to be only slightly smaller than that reported for low In-content GaxIn1xNyAs1y/GaAs films. Vurgaftman and Meyer [56] suggested x-dependent EN and V values for GaxIn1xNyAs1y and these values are summarized in Table 6.19. The higher-lying CPs in GaxIn1xNyAs1y have been studied using SE [233]. In strong contrast to the behavior of E and E þ , the higher-lying CPs such as E1 and E2 showed very weak liner nonlinearity with the N concentration. The temperature dependence of the fundamental absorption edge in GaxIn1xNyAs1y has also been studied by several authors [234–237] and found to exhibit weaker dependence than that observed in the N-free GaxIn1xAs matrix [234,235]. The pressure dependence of the fundamental absorption edge in GaxIn1xNyAs1y has been studied experimentally by several authors [139,234,238]. These results show a very much weaker pressure dependence than those observed in the N-free GaxIn1xAs alloy. (d) GaNPAs GaNxPyAs1xy were synthesized by N ion implantation into a GaPyAs1y epilayer (y ¼ 0 0.35) followed by pulsed-laser melting and rapid thermal annealing techniques [239]. As

186

PROPERTIES OF SEMICONDUCTOR ALLOYS

predicted from the BAC model, the incorporation of N split the CB in the bulk GaPyAs1y substrate, and relatively strong optical transitions from the VB to the lower (E) and upper (E þ ) conduction subbands were observed.

6.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs AlxGa1xPyAs1y lattice-matches to GaAs with x and y are given in Table 1.10. The AlxGa1xPyAs1y layers can also be grown on commercially available GaP0.39As0.61 epitaxial substrates. The lattice-matching relationship between x and y for the AlxGa1xPyAs1y/ GaP0.39As0.61 system can be written as y¼

0:079 þ 0:008x 0:2030:005x

ð0 x 1:0; 0:39 y 0:44Þ

ð6:24Þ

No detailed experimental data relating to the x-dependent band-gap energies in AlxGa1xPyAs1y have been published thus far. The E0, EgX and EgL values obtained from Equation (A.15) are plotted in Figure 6.41 as a function of x for (a) AlxGa1xPyAs1y/GaAs and (b) AlxGa1xPyAs1y/GaP0.39As0.61. The ternary bowing parameters are taken from Table 6.27, while the quaternary parameter DAlGaPAs is assumed to be zero. We can see that the E0 EgX crossing occurs at x 0.36 (Figure 6.41(a)) and at 0.07 (Figure 6.41(b)) (see also Table 6.28). 3. 5

3. 0

3.5 (a)

(b) 3.0 E0

E0, E gID (eV)

2. 0

1. 5

E0, E gID (eV)

E gL

2. 5

E gX E0

1. 0

2.5

E gL

2.0

E gX

1.5

1.0

0. 5

0.5 Alx Ga1-x Py As1-y /GaAs

0 0

0.2

0.4

0.6 x

Alx Ga1-x Py As1-y /GaPAs 0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.41 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlxGa1xPyAs1y/ GaAs and (b) AlxGa1xPyAs1y/GaP0.39As0.61 calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaPAs ¼ 0 eV

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

187

Table 6.28 Energy for the fundamental absorption edge (Eg) in III–V quaternaries at 300 K. The expression gives the quadratic fit of Equation (A.15) with DABCD ¼ 0 eV Quaternary

Substrate

Eg

Expression (eV)

AlxGa1xPyAs1y

GaAs

E0 EgX E0 EgX E0 EgX E0 EgX E0 EgX E0 EgX E0 EgL EgX E0 EgX E0 E0 E0 E0 E0 E0 EgX E0 E0

1.43 þ 1.50x þ 0.11x2 1.91 þ 1.93x þ 0.04x2 1.90 þ 1.42x þ 0.06x2 1.99 þ 0.18x þ 0.03x2 0.72 þ 1.46x þ 0.06x2 1.05 þ 0.54x þ 0.05x2 0.77 þ 1.53x þ 0.09x2 1.19 þ 0.65x þ 0.01x2 0.68 þ 1.48x þ 0.07x2 1.03 þ 0.60x þ 0.04x2 0.30 þ 1.17x þ 0.77x2 1.33 þ 0.68x 0.36x2 0.88 þ 0.88x þ 0.63x2 1.45 þ 0.30x þ 0.44x2 1.53 þ 0.53x 0.21x2 0.359 þ 1.143x þ 0.722x2 1.37 þ 0.57x 0.26x2 1.43 þ 0.30y þ 0.18y2 0.75 þ 0.46y þ 0.14y2 0.28 0.16x þ 0.60x2 0.97 0.84x þ 0.64x2 0.359 0.415x þ 0.718x2 1.90 þ 0.57x þ 0.10x2 2.25 þ 0.09x 0.01x2 0.75 þ 0.68x þ 0.06x2 0.512 þ 0.030y 0.183y2

GaPAs AlxGa1xAsySb1y

GaSb InP InAs

AlxIn1xAsySb1y

GaSb InP

InAs GaxIn1xPyAs1y

(AlxGa1x)0.53In0.47P

GaAs InP GaSb InP InAs GaAs

(AlxGa1x)0.48In0.52As InPxAsySb1xy

InP InAs

GaxIn1xAsySb1y

Remark

0.48 x 1.0 0.48 x 1.0 0.48 x 1.0

a b c 0.47 x 1.0 d d e f

Quadratic-fit result of Equation (A.15) with DAlInAsSb ¼ 0.11 eV Fit-determined from Figure 6.44 c Fit-determined from Figure 6.47 d Fit-determined from Figure 6.49 e dit-determined from Figure 6.50 f Fit-determined from Figure 6.51 a b

(b) AlGaAsSb AlxGa1xAsySb1y can be grown lattice-matched to GaSb, InP and InAs. The corresponding x and y relationships are presented in Table 1.10. This material system is attractive for optoelectronic applications in the near-IR wavelength range. However, very little data have so far been available on the composition-dependent band-gap energies in this alloy system. Herrera-Perez et al. [240] grew LPE-AlxGa1xAsySb1y layers (x ¼ 0.27, y ¼ 0.02) on GaSb (100) and determined from PR measurements the energy gaps to be 1.05 eV. Yacobi et al. [241] also obtained an absorption edge of 0.975 eV for (x, y) ¼ (0.15, 0.13) using a photothermal method. More recently, Saadallah et al. [189] undertook a photothermal study on an MBE-AlxGa1xAsySb1y/GaSb layer (x ¼ 0.70, y ¼ 0.08) and obtained an absorption edge

188

PROPERTIES OF SEMICONDUCTOR ALLOYS

of 1.57 eV. These data are plotted in Figure 6.42(a). The solid and dashed lines show the results calculated using Equation (A.15) together with the ternary bowing parameters shown in Table 6.27 and assuming DAlGaAsSb ¼ 0 eV. The quadratic fits of these curves are summarized in Table 6.28. Filho et al. [242] measured the temperature-dependent PL peak energies for an MBEAlxGa1xAsySb1y/InP layer (x ¼ 0.12, y ¼ 0.51) at T ¼ 10 180 K. By extrapolating these data, we can estimate the PL peak to be 0.89 eVat 300 K. This data is shown in Figure 6.42(b), together with the calculated data from Equation (A.15) (see also Table 6.28). The calculated E0, EgX and EgL values versus x curves for AlxGa1xAsySb1y/InAs in Figure 6.42(c) are very similar to those in Figure 6.42(a). This is not surprising in view of the near equality of the InAs and GaSb lattice parameters. Yacobi et al. [241] found the As composition for AlxGa1xAsySb1y at x ¼ 0.15 grown on GaSb substrate to be y ¼ 0.13. However, the exact lattice-matching relationship suggests that Yacobi’s sample (x, y) ¼ (0.15, 0.13) has y composition closely lattice-matched to InAs (y ¼ 0.10) rather than to GaSb (y ¼ 0.01). This data is, therefore, not only shown in Figure 6.42(a) but also in Figure 6.42(c). 2.5

2.5

(a)

2.5

(b)

2.0

(c)

2.0

2.0

E0,E gID (eV)

E gL

1.5

E gL

E gL E gX

1.0

E gX

1.5 1.0

E0

1.5 1.0

E0

0.5

E0

0.5 Alx Ga1-x Asy Sb1-y /GaSb

0 0

E gX

0 0.2 0.4 0.6 0.8 1.0 0 x

0.5 Alx Ga1-x Asy Sb1-y /InP

0 0.2 0.4 0.6 0.8 1.0 0 x

Alx Ga1-x Asy Sb1-y /InAs

0.2 0.4 0.6 0.8 1.0 x

Figure 6.42 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlxGa1xAsySb1y/ GaSb, (b) AlxGa1xAsySb1y/InP and (c) AlxGa1xAsySb1y/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaAsSb ¼ 0 eV

No clear bowing can be seen for E0 in Figure 6.42. The Al0.5Ga0.5AsxSb1x layers (x ¼ 0.3 0.7) grown on GaAs by MBE have also been studied by PL [243]. A discrepancy of up to 0.2 eV from the predicted value using the established formalism indicates that an extra bowing factor needs to be included in the E0 versus x expression for this quaternary system. The temperature dependence of the fundamental absorption edges has been studied for AlxGa1xAsySb1y/GaSb (x ¼ 0.27, y ¼ 0.02) [240] and AlxGa1xAsySb1y/InP (x ¼ 0.12, y ¼ 0.51) [242]. The Varshni parameters for AlxGa1xAsySb1y/GaSb were a ¼ 3.6 104 eV/K and b ¼ 78 K [240], which are considerably smaller than the endpoint binary values a ¼ (3.6 5.5) 104 eV/K and b ¼ 204 234 K [1]. (c) AlInAsSb AlxIn1xAsySb1y can be grown lattice-matched to GaSb, InP and InAs (Table 1.10). However, no detailed study has been carried out on AlxIn1xAsySb1y lattice-matched to GaSb and InP.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

189

There is only one study by Charykov et al. [244] which reports PL measurements on LPEAlxIn1xAsySb1y/InAs epilayers. The composition range investigated corresponds to a wavelength from 3 (x ¼ 0) to 2.5 mm (x ¼ 0.08). The solid and dashed lines in Figure 6.43 show the calculated E0, EgX and EgL gaps as a function of x for AlxIn1xAsySb1y lattice-matched to GaSb, InP and InAs. These are obtained from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlInAsSb ¼ 0 eV. The quadratic fits of these curves are summarized in Table 6.28. The solid circles in Figure 6.43(c) represent the experimental data taken from Charykov et al. [244]. The direct–indirect crossover occurs at xc ¼ 0.77 in (a), 0.70 in (b) and 0.77 in (c). 2.5

2.5

(a)

2.5

(c)

(b)

2.0

2.0

2.0

E0, E gID (eV)

E gX

1.5

E gX

1.5

E gL

1.5

E gX

E0

1.0

E gL

E0

0.5

1.0 0.5

AlxIn1-xAsySb1-y /GaSb

0 0

1.0

0.2 0.4 0.6 0.8 1.0 x

E0

0.5 AlxIn1-xAsySb1-y /InP

0 0

E gL

0.2 0.4 0.6 0.8 1.0 x

AlxIn1-xAsySb1-y /InAs

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.43 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlxIn1xAsySb1y/ GaSb, (b) AlxIn1xAsySb1y/InP and (c) AlxIn1xAsySb1y/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlInAsSb ¼ 0 eV. The experimental data in (c) are taken from Charykov et al. [244]

(d) GaInPAs A number of experimental studies have been published on E0 versus composition for GaxIn1xPyAs1y quaternary alloy. These studies concentrated on the technologically important compositions which have lattice parameters equal to that of InP [245]. GaxIn1xPyAs1y can also be grown lattice-matched to GaAs. However, not very much is known about GaxIn1xPyAs1y/GaAs. Shirakata et al. [246] performed ER measurements on LPE-grown GaxIn1xPyAs1y/GaAs with y ¼ 0.70 and 0.96. These data are plotted versus y in Figure 6.44(a). The experimental data for GaxIn1xPyAs1y/InP are gathered from various sources and plotted in Figure 6.44(b). The solid and dashed lines in Figure 6.44 are obtained from Equation (A.15) using the ternary bowing parameters in Table 6.27 and inputting DAlInAsSb ¼ 0.11 (E0) and 0 eV (EgX and EgL ). The quaternary parameter DAlInAsSb ¼ 0.11 eV is taken from Donati et al. [247]. This parameter explains the E0 data plotted in Figure 6.44(a), but not that in Figure 6.44(b). The heavy solid line in Figure 6.44(b) shows the quadratic least-squares fit of E0. The bowing parameter of c ¼ 0.14 eV is determined from this fit (Table 6.28). The higher-lying CPs, such as E0 þ D0, E1, E1 þ D1, E00 and E2, for GaxIn1xPyAs1y/InP have been investigated by many authors [245,248,249]. The recommended higher-lying CPs are listed in Table 6.29 (see also Figure 6.45(a)).

190

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.5

2.5 (a)

2.0

EgX E0,E gID (eV)

E0,E gID (eV)

2.0

Gax In1-x Py As1-y /InP

EgL

E0

1.5

1.0

EgL

EgX 1.5 E0 1.0

Gax In1-x Py As1-y /GaAs 0.5

0

(b)

0.2 0.4 0.6 0.8 1.0 y

0.5 0

0.2 0.4 0.6 0.8 1.0 y

Figure 6.44 Energies of the lowest direct E0 and indirect gaps EgID versus y for (a) GaxIn1xPyAs1y/ GaAs and (b) GaxIn1xPyAs1y/InP calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DGaInPAs ¼ 0.11 (E0) and 0 eV ðEgX Þ and ðEgL Þ. The heavy solid line in (b) shows the quadratic least-squares fit listed in Table 6.28

6

6

6

(a) E 0′

5

E gD (eV)

4

E1+∆1 E1

2

E0+∆0 1

E1

3

E0+∆0

2

E0

0

5

E2

4

E 0′

3 2 1

1 Gax In1-x Py As1-y /InP

0

E2

5 4

3

(AlxGa1-x)0.48In0.52As/InP

(b)

(AlxGa1-x)0.53In0.47P/GaAs

0

0.2 0.4 0.6 0.8 1.0 0 y

0

0.2 0.4 0.6 0.8 1.0 0 x

E1+∆1 E1

E0+∆0 E0

(c)

0.2 0.4 0.6 0.8 1.0 x

Figure 6.45 Energies of the higher-lying CPs versus y or x for (a) GaxIn1xPyAs1y/InP, (b) (AlxGa1x)0.53In0.47P/GaAs and (c) (AlxGa1x)0.48In0.52As/InP. The functional forms are summarized in Tables 6.28 and 6.29

The temperature dependence of E0 for GaxIn1xPyAs1y/InP has been studied by several authors [245]. The experimental dE0/dT versus y data are shown in Figure 6.46(a). These data give the slowly varying function of dE0/dT versus y (in 104 eV/K)

dE0 ¼ 3:6 þ 0:5y dT

ð6:25Þ

The pressure coefficient dE0/dp for GaxIn1xPyAs1y/InP has been studied by several authors [245]. These results are summarized in Figure 6.46(b). The corresponding y dependence is written as (in 102 eV/GPa)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

191

Table 6.29 Energies for the higher-lying CPs in some III–V quaternaries at 300 K Quaternary

Substrate

CP

GaxIn1xPyAs1y

InP

E0 þ E1 E1 þ E00 E0 þ E1 E2 E0 þ E1 E1 þ E00 E2

(AlxGa1x)0.53In0.47P

GaAs

(AlxGa1x)0.48In0.52As

InP

Expression (eV) D0

1.08 2.56 2.85 4.42 1.98 3.23 4.80 1.10 2.55 2.83 4.36 4.74

D1 D0 D0 D1

dE0 ¼ 11:33:0y dp

þ þ þ þ þ þ þ þ þ þ þ þ

0.30y þ 0.08y2 0.34y þ 0.27y2 0.25y þ 0.19y2 0.27y þ 0.01y2 0.62x þ 0.10x2 0.37x þ 0.09x2 0.02x 0.64x þ 0.18x2 0.36x þ 0.11x2 0.39x þ 0.08x2 0.69x 0.48x2 0.15x 0.13x2

ð6:26Þ

(e) GaInAsSb Figure 6.47 shows E0, EgX and EgL versus x for GaxIn1xAsySb1y lattice-matched to GaSb, InP and InAs. A distinguishing feature of GaxIn1xAsySb1y is the existence of a wide immiscibility range 0.24 < x < 0.75, which means that the alloy can be prepared only in a narrow range of compositions either adjoining GaSb (x ¼ 1.0) or InAs (x ¼ 0). The solid and dashed lines in Figure 6.47 are calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DGaInAsSb ¼ 0 eV.

6

15

(a) dE120 /dp (10-2 eV/GPa)

-dE0 /dT (10-4 eV/K)

5 4 3 2

6 3

1 0

9

GaxIn1-xPyAs1-y/InP 0

0.2 0.4 0.6 0.8 1.0 y

(b) 0 0

0.2 0.4 0.6 0.8 1.0 y

Figure 6.46 (a) Temperature and (b) pressure coefficients of E0 as a function of y for GaxIn1xPyAs1y/ InP. The solid lines in (a) and (b) are obtained from Equations (6.25) and (6.26), respectively

192

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.0

2.0 Gax In1-x Asy Sb1-y /GaSb

E0, E gID (eV)

1.5

2.0 Gax In1-x Asy Sb1-y /InP

1.5

1.5

E gX E gL

EgX

1.0

1.0

EgL E0

0.5

E0

0.5

(a)

0 0

EgX

1.0

EgL

0.5

Gax In1-x AsySb1-y /InAs

0 0.2 0.4 0.6 0.8 1.0 0 x

E0

(b)

(c)

0 0.2 0.4 0.6 0.8 1.0 0 x

0.2 0.4 0.6 0.8 1.0 x

Figure 6.47 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) GaxIn1xAsySb1y/ GaSb, (b) GaxIn1xAsySb1y/InP and (c) GaxIn1xAsySb1y/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DGaInAsSb ¼ 0 eV. The heavy solid line in Figure 6.47(a) shows the quadratic least-squares fit listed in Table 6.28

The open circles in Figure 6.47 show the experimental data taken from various sources [250– 254]. It can bee seen that Equation (A.15) shows reasonable agreement with the available experimental data. However, Figure 6.47(a) shows poor agreement. We, therefore, tried to least-squares fit these data using a quadratic function. The heavy solid line in Figure 6.47(a) shows this result. The determined bowing parameter is c ¼ 0.60 eV (Table 6.28). The temperature dependence of the G-valley gap E0 has been studied by Iyer et al. [255] and Mu~ noz et al. [256] for GaxIn1xAsySb1y grown on GaSb and by Gong et al. [257] for GaxIn1xAsySb1y grown on InAs. These results are shown in Figure 6.48. Although the data are somewhat sparse, they give values of dE0/dT 3.8 104 and 4.0 104 eV/K for samples grown on GaSb and InAs, respectively, near 300 K. 8 7

GaxIn1-xAsySb1-y

-dE0 /dT (10-4 eV/K)

6 5 on InAs 4 3

on GaSb

2 1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.48 Temperature coefficient dE0/dT as a function of x for GaxIn1xAsySb1y lattice-matched to GaSb and InAs

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

193

6.4.3 (III, III, III)–V Alloy (a) AlGaInP AlxGayIn1xyP has the largest direct band gap of any semiconductor lattice-matched to GaAs. There have been many reports on (AlxGa1x)0.53In0.47P/GaAs (see e.g. [258–260]). The open circles in Figure 6.49 represent the experimental data at 300 K. They are taken from various sources, e.g. Asami et al. [261], Cao et al. [262] and Adachi et al. [263]. Data for E0, EgX and EgL for (AlxGa1x)0.53In0.47P/GaAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaInP ¼ 0 eV have been plotted in Figure 6.49.

3.0

E gL

E0, E gID (eV)

2.5

E gX E0

2.0

(AlxGa1-x)0.53In0.47P/GaAs 1.5 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.49 Energies of the lowest direct E0 and indirect gaps EgID versus x for (AlxGa1x)0.53In0.47P/ GaAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaInP ¼ 0 eV. The heavy solid lines show the quadratic least-squares fit listed in Table 6.28

Equation (A.15) predicts that the G–X crossover occurs at xc ¼ 0.55. However, excellent agreement can be never achieved with the experimental data even if DAlGaInP 6¼ 0 eV is introduced into Equation (A.15). We, therefore, fit the experimental E0 and EgX data using a quadratic function with respect to x. The heavy solid lines in Figure 6.49 show these results (see also Table 6.28) and predict that the G–X crossover point will be at xc ¼ 0.64. No experimental data has, however, been reported on the G–X crossover point. The higher-lying CPs as a function of x for (AlxGa1x)0.53In0.47P/GaAs have been determined using various techniques, such as ER [261,263], TR [264] and SE [260,264,265]. The E0 þ D0, E1 and E2 energies versus x for (AlxGa1x)0.53In0.47P/GaAs have been plotted in Figure 6.45(b). They are obtained by averaging the published experimental data and are summarized in Table 6.29.

194

PROPERTIES OF SEMICONDUCTOR ALLOYS

The pressure dependence of E0 for (AlxGa1x)0.53In0.47P/GaAs has been investigated by several authors [266,267]. The experimental data reported by Harada et al. [267] can be written as dE0 dE0 ð0Þ ¼ ð10:29xÞ dp dp

ð6:27Þ

where dE0(0)/dp ¼ 9.5 eV/GPa is the Ga0.5In0.5P (x ¼ 0) value estimated from the linear interpolation between GaP and InP [1]. (b) AlGaInAs AlxGayIn1xyAs can be relatively easily grown on InP by MBE. This alloy system can also be prepared by MOCVD [268]. The E0, EgX and EgL gaps for (AlxGa1x)0.48In0.52As/InP are shown in Figure 6.50. The alloy system remains a direct gap material over the whole composition range 0 x 1.0. The open circles in Figure 6.50 represent the experimental E0 data taken from various sources (see e.g. [268–271]). These data are found to be slightly smaller than those calculated from Equation (A.15) assuming DAlGaInAs ¼ 0 eV. The heavy solid line in Figure 6.50 represents the quadratic least-squares fit (Table 6.28).

2.0

E gX

E0, E gID (eV)

1.5 EgL 1.0

E0

0.5 (AlxGa1-x)0.48In0.52As/InP 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.50 Energies of the lowest direct E0 and indirect gaps EgID versus x for (AlxGa1x)0.48In0.52As/ InP calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaInAs ¼ 0 eV. The heavy solid line shows the quadratic least-squares fit listed in Table 6.28

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

195

The higher-lying CPs in (AlxGa1x)0.48In0.52As/InP have been studied using ER [272] and SE [273]. The E0 þ D0, E1, E1 þ D1, E00 and E2 versus x data for (AlxGa1x)0.48In0.52As/InP as determined by ER [272] has been plotted in Figure 6.45(c). The corresponding expressions are summarized in Table 6.29.

6.4.4 III–(V, V, V) Alloy InPxAsySb1xy/InAs is the only quaternary system that has been well studied in the literature. The E0 versus y data for InPxAsySb1xy/InAs are shown in Figure 6.51. They are taken from various sources [213,274–276]. The solid and dashed lines also show the E0, EgX and EgL versus y curves obtained from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DInPAsSb ¼ 0 eV. The heavy solid line is obtained from the quadratic least-squares fit. This fit gives considerable upward bowing of c ¼ 0.183 eV for E0 (Table 6.28).

2.0

E gX

E0,E gID (eV)

1.5 E gL 1.0

E0 0.5 InPxAsySb1-x-y /InAs 0

0

0.2

0.4

y

0.6

0.8

1.0

Figure 6.51 Energies of the lowest direct E0 and indirect gaps EgID versus y for InPxAsySb1xy/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DInPAsSb ¼ 0 eV. The heavy solid line shows the quadratic least-squares fit listed in Table 6.28

The higher-lying CPs, E0 þ D0, E1 and E1 þ D1, in InPxAsySb1xy/InAs have been determined using ER [274,275]. Like E0, these CPs show no strong dependence on alloy composition. The temperature dependence of E0 has also been determined to be (2.2–2.9) 104 eV/K for 0.46 y 1.0 [275], suggesting little dependence on alloy composition.

196

PROPERTIES OF SEMICONDUCTOR ALLOYS

6.4.5 Summary The lowest direct (E0) and indirect gaps (EgX ) for some III–V quaternary alloys lattice-matched to (a) GaAs, (b) GaSb, (c) InP and (d) InAs are summarized in Figure 6.52. The limits of applicability of the linear interpolation scheme using the binary data are apparent. The rationalized biquadratic interpolation algorithm, Equation (A.15), can be safely used to estimate the band-gap energies in quaternary alloys. However, it tends to give energies that are smaller (Figures 6.44, 6.47 and 6.50) or larger than the experimental data (Figures 6.49 and 6.51). These poorer fits can be improved to some extent, if the nonzero DABCD parameter is inserted into Equation (A.15). For example, introducing DGaInPAs ¼ 0.5 eV into Equation (A.15) improves the fit considerably, as demonstrated in Figure 6.53. It is, however, very difficult to explain the origin of such large upward bowing in this alloy system (GaxIn1xPyAs1y/InP). The alloying effect in certain types of (III, III)–(V, V) quaternaries may be a secondary effect of the relatively strong cation–cation and anion–anion sublattice disorders which occur in ternary alloys. The triple cation or anion disorder effect may also be much smaller in alloys of the type (III, III, III)–Vor III–(V, V, V). We can, therefore, expect that Equation (A.15) will become a good tool for obtaining reliable quaternary parameters when more exact ternary bowing parameters, which can be introduced into Equation (A.15), are required.

2.5

(b) GaSb

(c) InP

(d) InAs

E0,E gX (eV)

2.0 1.5 1.0 0.5

(a) GaAs 0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x (y) x x (y) x (y) GaxIn1-xPyAs1-y (y) (AlxGa1-x)0.53In0.47P

AlxGa1-xAsySb1-y AlxIn1-xAsySb1-y GaxIn1-xAsySb1-y

AlxGa1-xAsySb1-y AlxIn1-xAsySb1-y GaxIn1-xPyAs1-y (y) GaxIn1-xAsySb1-y (AlxGa1-x)0.48In0.52As

AlxGa1-xAsySb1-y AlxIn1-xAsySb1-y GaxIn1-xAsySb1-y InPxAsySb1-x-y (y)

Figure 6.52 Energy of the lowest band gap E0 or EgX versus x (or y) for some IIIV quaternary alloys lattice-matched to (a) GaAs, (b) GaSb, (c) InP and (d) InAs. These curves are calculated from the data in Table 6.28

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

197

1.4

1.2

E0 (eV)

DGaInPAs =+1.5eV 1.0

0.8

-0.5 eV Gax In1-x Py As1-y /InP

0.6 0

0.2

0.4

y

0.6

0.8

1.0

Figure 6.53 Lowest band-gap energy E0 versus y for GaxIn1xPyAs1y/InP at 300 K. The solid lines are calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and varying DGaInPAs from 0.5 to þ 1.5 eV in steps of 0.5 eV

6.5 II–VI SEMICONDUCTOR ALLOY 6.5.1 (II, II)–O Ternary Alloy (a) BeZnO Beryllium chalcogenides attracted considerable attention because they exhibit covalent bonding, and appear to have very large band gaps. However, their optical and electronic properties have not yet been fully clarified. Both BeO and ZnO usually crystallize in the wurtzite structure. BeO has a wide band gap (E0 ¼ 10.6 eV). Studies on BexZn1xO are very limited. Ryu et al. [277] deposited BexZn1xO layers on sapphire substrates using a hydride beam deposition method. They measured the transmittance spectra at 300 K and obtained E0 for 0 x 0.69. More recently, Han et al. [278] used the same crystal growth and measurement techniques, and obtained E0 up to x ¼ 0.28. These data are shown in Figure 6.54(a) (open circles [277], solid circles [278]). The solid line shows a rough fit of these data using the quadratic function shown in Table 6.30. (b) MgZnO MgO is the prototype of an ionic semiconductor crystallizing in the rocksalt structure, whereas ZnO crystallizes in the wurtzite structure. There have been many studies on the electronic energyband structure of MgxZn1xO. The E0 versus x data taken from various sources (see e.g. [279– 283]) are shown in Figure 6.54(b). It can be seen that the E0 data for x 0.5 are a good fit with the linear function of x, while those for x > 0.4 show quadratic dependence on x. The corresponding expressions are listed in Table 6.30. The wurtzite–cubic mixed phase region occurs at around x 0.4.

198

PROPERTIES OF SEMICONDUCTOR ALLOYS 12

8

(b) MgxZn1-xO

(c) ZnxCd1-xO

7

10 wurtzite

9 E0 (eV)

4.0

(a) BexZn1-xO

11

3.5 rocksalt

6

8

3.0

7

rocksalt

5 wurtzite

6

2.5

4

5 4

mixed phase

3

3 2

2 0

0.2 0.4 0.6 0.8 1.0 x

2.0 wurtzite

1.5 0

0.2 0.4 0.6 0.8 1.0 x

0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.54 Energy of the E0 gap versus x for some (II, II)–O ternaries at 300 K: (a) BexZn1xO, (b) MgxZn1xO and (c) ZnxCd1xO. The solid lines represent the calculated results using the data in Table 6.30

The composition dependence of the higher-lying CPs in w-MgxZn1xO has been studied using SE [280]. E1 and E2 energies were observed at 7 and 9 eV, respectively, and showed little dependence on x. The pressure dependence of E0 has been measured using a diamond anvil cell for p up to 10 GPa [284]. The experimental pressure coefficient dE0/dp increased at a rate of 40x meV/GPa (0 x 0.13). (c) ZnCdO There have been a few reports on ZnxCd1xO [285,286]. The E0 versus x data measured by Ishihara et al. [285] (solid circles) and Wang et al. [286] (open circles) have been plotted in Figure 6.54(c) These plots show that E0 in the wurtzite region varies quadratically with x (0.2 x 1.0, see Table 6.30). The E0 value in the rocksalt region decreases with decreasing x. The E0 versus x data at 2.1 K have been determined using PL [287]. The temperature dependence of E0 has also been established by Makino [279] for T ¼ 5–300 K (x ¼ 0.01) and Wang et al. [286] for T ¼ 6–300 K (x ¼ 0.022, 0.09 and 0.157), illustrating nearly the same behavior as that for ZnO [279].

6.5.2 (II, II)–S Ternary Alloy (a) MgZnS Under normal conditions MgS crystallizes in the rocksalt structure, whereas ZnS crystallizes either in the wurtzite or zinc-blende structure. ZnS has the largest band gap among II–VI semiconductors except for Be- and Mg-chalcogenides. The E0 gap in w-MgxZn1xS has been investigated by means of optical absorption [288]. The samples used were grown on (0001)sapphire substrates by PLD. These data are shown in Figure 6.55(a) by the solid circles. It can

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

199

Table 6.30 Energy for E0 in some II–VI ternaries and quaternaries at 300 K. w ¼ wurtzite; rs ¼ rocksalt; zb ¼ zinc-blende Alloy BexZn1xO MgxZn1xO ZnxCd1xO MgxZn1xS ZnxCd1xS ZnxHg1xS CdxHg1xS BexZn1xSe BexCd1xSe MgxZn1xSe MgxCd1xSe ZnxCd1xSe CdxHg1xSe BexZn1xTe MgxZn1xTe MgxCd1xTe ZnxCd1xTe ZnxHg1xTe CdxHg1xTe ZnOxS1x ZnSxSe1x ZnSxTe1x ZnSexTe1x CdSxSe1x CdSxTe1x CdSexTe1x MgxZn1xSySe1y/GaAs MgxZn1xSeyTe1y/InP BexMgyZn1xySe/GaAs MgxZnyCd1xySe/InP

E0 (eV) 3.4 2.1x þ 9.3x2 3.4 þ 2.3x 7.2 5.0x þ 5.6x2 1.76 0.11x þ 1.75x2 3.81 þ 0.65x 3.75 þ 0.80x 2.460 þ 0.439x þ 0.827x2 2.501 þ 0.328x þ 0.921x2 0.040 þ 2.770x þ 0.996x2 0.040 þ 2.541x 2.721 þ 1.846x þ 1.033x2 1.675 þ 0.925x þ 3.000x2 2.721 þ 0.679x þ 0.600x2 1.675 þ 2.125x þ 0.200x2 1.751 þ 2.349x 1.675 þ 0.659x þ 0.387x2 0.08 þ 1.57x 2.27 þ 1.83x 2.27 þ 0.67x þ 0.46x2 1.51 þ 1.35x þ 0.54x2 1.51 þ 0.45x þ 0.31x2 0.15 þ 1.96x þ 0.46x2 0.15 þ 1.45x þ 0.21x2 3.75 4.85x þ 4.50x2 2.721 þ 0.425x þ 0.580x2 2.270 2.294x þ 3.750x2 2.270 1.049x þ 1.500x2 1.751 þ 0.050x þ 0.700x2 1.51 0.85x þ 1.80x2 1.560 0.859x þ 1.800x2 1.510 0.673x þ 0.838x2 2.749 þ 1.340x þ 0.650x2 2.13 þ 1.59x þ 0.37x2 2.79 þ 1.44y þ 1.74y2 2.11 þ 1.57x þ 0.40x2

Remark w (0 x 1.0) w (0 x 0.5) rs (0.4 x 1.0) w (0.2 x 1.0) zb (0 x 0.25), T ¼ 10 K w (0 x 0.25) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) w (0.6 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 0.32) w (0 x 1.0) zb (0 x 1.0) zb (0 x 0.8) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) zb (0 x 0.5) zb (0 x 0.84) zb (0 y 0.67) zb (0 x 0.83)

be seen that E0 increases almost linearly at a rate of 0.8x eV from E0 ¼ 3.75 eV at x ¼ 0 (wZnS). The detailed expression is given in Table 6.30. The zinc-blende MgxZn1xS layers for x up to 0.24 have been grown on GaP(100) by MBE [289]. The E0 gaps for these layers are determined by low-temperature (10 K) PL measurements. These results are shown in Figure 6.55(a) by the open circles. As in the case of w-MgxZn1xS, the E0 gap in c-MgxZn1xS increases at a rate of 0.7x eV from E0 ¼ 3.81 eVat x ¼ 0 (c-ZnS). From the extrapolation scheme E0 4.5 eV for c-MgS is estimated to occur at 10 K.

200

PROPERTIES OF SEMICONDUCTOR ALLOYS 4.1

3.8 3.6

E0 (eV)

zinc-blende 4.0 (T=10 K)

3.4 3.2

4

(b) ZnxCd1-xS

3

(c) ZnxHg1-xS 3

wurtzite cubic

(d) CdxHg1-xS 2 zincblende

2

3.9

1 3.0 wurtzite

wurtzite

1

2.8

3.8

0

(a) MgxZn1-xS

2.6

0 zinc-blende

mixed phase

3.7 2.4 -1 -1 0 0.1 0.2 0.3 0.4 0.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x x

Figure 6.55 Energy of the E0 gap versus x for some (II, II)–S ternaries at 300 K: (a) MgxZn1xS, (b) ZnxCd1xS, (c) ZnxHg1xS and (d) CdxHg1xS. The solid and dashed lines represent the calculated results using the data in Table 6.30

(b) ZnCdS ZnxCd1xS can be grown both in the wurtzite and zinc-blende structures. The E0 versus x data for w-ZnxCd1xS reported in the literature [2–293] are shown in Figure 6.55(b). The experimental data largely scatter. The solid line shows the least-squares fit of these data (see Table 6.30). This fit gives a bowing parameter of c 0.921 eV. Yokogawa et al. [294] estimated c 0.827 eV for E0 in c-ZnxCd1xS. Introducing this value into Equation (A.5), the composition dependence of E0 for c-ZnxCd1xS can be calculated. The dashed line in Figure 6.55(b) represents the result of this calculation (see also Table 6.30). The temperature coefficient of E0 for w-ZnxCd1xS has been studied by means of electroabsorption spectroscopy [295]. The experimental dE0/dT is in the range of (3.8–6.0) 104 eV/K for x ¼ 0–1.0. The pressure coefficient dE0/dp in w-ZnxCd1xS has also been determined for p up to 15 GPa [291]. The linear pressure coefficient, when plotted against the Cd concentration, displays a slow decrease up to 25 at% at which concentration a sudden drop appears. This behavior is reminiscent of ‘percolation-type’ phenomena. (c) ZnHgS The complete solid solution was obtained throughout the whole range for the ZnS–HgS alloy system [296]. The reflectance measurements revealed that the zinc-blende ZnxHg1xS alloy appears to show a nearly linear increase of E0 from x 0.44 to 1.0. These results are shown in Figure 6.55(c) [296]. The solid line shows the quadratic fit of these data and those for x ¼ 0 and 1.0 (see also Table 6.30). (d) CdHgS CdS and HgS form solid solutions over the whole range, but the crystal structure depends on the composition. The zinc-blende solid solution c-CdxHg1xS is obtained in the x ¼ 0–0.4 range, while the wurtzite solid solution w-CdxHg1xS is obtained for x 0.6. The cubic and wurtzite

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

201

structures can be present in the x ¼ 0.4–0.6 range. As expected, the ratio of cubic to wurtzite solid solution increases continuously with increasing HgS concentration [296,297]. The dependence of E0 on x for CdxHg1xS is shown in Figure 6.55(d) [296]. We can see that the E0 versus x data are satisfactorily interpreted by the linear interpolation scheme between the CdS (2.541 eV) and HgS values (0.04 eV), as shown by the solid line.

6.5.3 (II, II)–Se Ternary Alloy (a) BeZnSe Figure 6.56(a) shows the E0 versus x data for BexZn1xSe obtained using SE by Wilmers et al. [298] (solid circles) and Bukaluk et al. [299] (open circles). The solid line represents the quadratic least-squares fit of these data. The bowing parameter c is determined to be 1.033 eV (Table 6.30). 6

6

(a) BexZn1-xSe 5

E0, E gX (eV)

5

4 4 3

4.5

(b) BexCd1-xSe

EgX

(c) MgxZn1-xSe 4.0

zinc-blende

EgX

3.5 3

E0

2 zinc-blende

3.0 E0

EgX E0

zinc-blende

2 1 2.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x 3.0 2 4 (d) MgxCd1-xSe (e) ZnxCd1-xSe (f) CdxHg1-xSe

E0 (eV)

wurtzite

2.5

3

2

5 4 3 2 zb 1 0 0.5 1.0

2.0

zinc-blende

1

0

zinc-blende

wurtzite mixed phase

1 1.5 -1 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x

Figure 6.56 Energy of the E0 gap versus x for some (II, II)–Se ternaries at 300 K: (a) BexZn1xSe, (b) BexCd1xSe, (c) MgxZn1xSe, (d) MgxCd1xSe, (e) ZnxCd1xSe and (f) CdxHg1xSe. The solid lines represent the calculated results using the data in Table 6.30. The dashed lines in (a)–(c) show the x dependence of EgX obtained by the linear interpolation between the endpoint binary data in Table 6.1. The dotted line in (d) represents the liner least-squares fit, which predicts a value of E0 3.8 eV for w-MgSe (x ¼ 1.0). The inset in (d) shows the x dependence of E0 in c-MgxCd1xSe (see also Table 6.30)

Beryllium chalcogenides BeX (X ¼ S, Se, Te) are characterized by an indirect band gap with the CB minimum lying at the X point [300]. The direct and indirect gaps of these materials are listed in Table 6.1. The dashed line in Figure 6.56(a) shows the x dependence of EgX for

202

PROPERTIES OF SEMICONDUCTOR ALLOYS

BexZn1xSe obtained by the linear interpolation between ZnSe (x ¼ 0) and BeSe (x ¼ 1.0). We can expect the G–X crossover to occur at x 0.4. This agrees with an abrupt drop in the main PL peak intensity at x 0.45 [301,302]. The SE spectra for BexZn1xSe have been measured in the 2–30 eV range [298], the 1.25–5 eV range [299] and the 1.5–6.0 eV range [303]. The higher-lying CPs assigned to E0 þ D0, E1, E1 þ D1, E2, E00 and E10 can be seen [298] and with increasing Be content their spectral positions are systematically shifted toward higher energies. Each CP has a different slope dEg/dx, E0 and E0 þ D0 having the steepest slope and, as a result, having the largest bowing parameter. The highest CP peak is at 8.5 eV (E10 ) [298]. (b) BeCdSe The zinc-blende-type BexCd1xSe alloy can be epitaxially grown on III–V semiconductor substrates. E0 values for c-BexCd1xSe epilayers grown on GaAs(100) [304] and on InP(100) have been reported [305,306]. The experimental data obtained from these studies are shown in Figure 6.56(b). The solid line shows a quadratic dependence of E0 on x (Table 6.30). The dashed line also shows the predicted EgX values obtained by the linear interpolation between c-CdSe (x ¼ 0) and BeSe (x ¼ 1.0). The G–X crossover is expected to occur at x 0.8. The E0 value in w-BexCd1xSe has also been measured by Huang et al. [306] and Wronkowska et al. [307]. (c) MgZnSe Bulk MgxZn1xSe crystals grown by the Bridgman method are known to show the sphalerite–wurtzite phase transition at x ¼ 0.185 0.03 [308]. On the other hand, c-MgxZn1xSe epilayer can be grown over the whole alloy range (0 x 1.0). The E0 versus x data for cMgxZn1xSe reported in the literature [309–312] are shown in Figure 6.56(c). The quadratic least-squares fit produces a bowing of c 0.600 eV for E0 (Table 6.30). The dashed line represents the x dependence of EgX obtained by the linear interpolation between ZnSe (x ¼ 0) and MgSe (x ¼ 1.0). It can be seen that the G–X crossover occurs at x 0.55. No experimental determination has, however, been reported until now. The higher-lying CPs in c-MgxZn1xSe have been studied using SE for x 0.37 [303] and x 0.21 [311]. The E0 þ D0, E1 and E1 þ D1 CPs are reported to increase almost linearly with increasing x. The temperature dependence of E0 has been studied for both c-MgxZn1xSe [313,314] and w-MgxZn1xSe [315]. The experimental data have been analyzed using semi-empirical formulas, such as the Varshni and P€assler formulas [1]. An anomalous temperature dependence, i.e. showing a positive temperature coefficient at T 70 K, has also been found in bulk w-MgxZn1xSe crystals grown by a closed-tube sublimation method and analyzed as originating from a volume dilution effect due to deep-level defects [315]. (d) MgCdSe Under normal conditions bulk MgxCd1xSe crystallizes in the wurtzite structure. The E0 versus x data for w-MgxCd1xSe obtained from Wronkowska et al. [316] (open circles), Firszt et al. [317] (open triangles) and Kim et al. [318] (solid circles) are shown in Figure 6.56(d); the experimental data scatter largely. The dotted line represents the linear least-squares fit of these data, which gives a change of E0 at a rate of dE0/dx ¼ 2.071 eV and predicts a value of E0 3.8 eV for w-MgSe. This value is considerably smaller than that of c-MgSe (E0 ¼ 4.0 eV,

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

203

Table 6.1). In III–Vand II–VI semiconductors, the wurtzite polytype usually has a larger E0 gap than the zinc-blende polytype (Tables 6.1 and 6.2). Thus, the E0 value for w-MgSe should be larger than that for c-MgSe (4.0 eV). The solid line in Figure 6.56(d) shows the linearly interpolated result assuming E0 ¼ 4.1 eV for w-MgSe. The E0 versus x data for c-MgxCd1xSe layers (x 0.32) grown on InAs(100) have been determined using low-temperature (77 K) PL [319]. The bowing parameter c 0.2 eV is estimated from this study. The inset in Figure 6.56(d) shows the E0 versus x dependence at 300 K for c-MgxCd1xSe obtained by introducing c ¼ 0.200 eV into Equation (A.5) (see also Table 6.30). The composition dependence of E0 at 11 K for w-MgxCd1xSe has been determined from PL measurements [320]. The temperature dependence of E0 has also been reported by several authors [318,321]. Using SE, Wronkowska et al. [316] determined the higher-lying CPs for w-MgxCd1xSe. However, they explained these data using the notations of the zinc-blende lattice (E0 þ D0 and E1), not those of the wurtzite lattice (E0a and E1a (a ¼ A, B or C); see Adachi [1]). (e) ZnCdSe ZnxCd1xSe is commonly used as QW material in ZnSe-based devices. In the bulk form, ZnxCd1xSe has the zinc-blende structure at 0.7 x 1.0, the wurtzite structure at 0 x 0.3 and their mixed phases at 0.3 x 0.7 [322]. On the other hand, MBE-grown ZnxCd1xSe layers on GaAs(100) result in films of the zinc-blende structure over the whole composition range. The E0 versus x data for c-ZnxCd1xSe/GaAs(100) epilayers grown by MBE are shown in Figure 6.56(e) [323–326]. The solid line shows the quadratic least-squares fit of these data (see also Table 6.30). The higher-lying CPs in c-ZnxCd1xSe epilayers at 0 x 1.0 have been studied using SE in the 1.5–6.0 eV range [324]. The E0 þ D0, E1 and E1 þ D1 CPs have been observed and found to increase with increasing x. The corresponding bowing parameters are found to be c ¼ 0.38 (E0 þ D0), 0.467 (E1) and 0.351 eV (E1 þ D1). The temperature dependence of E0 for c-ZnxCd1xSe layers grown by MBE has been determined by several authors [326–328]. Using SE, Lee et al. [326] obtained an expression that allows E0 to be obtained for any composition and temperature within the ranges 0 x 0.34 and 25 T 260 C. The E0 versus T variation has also been determined by ER in the range 25 T 400 K for x ¼ 0.56 [327] and by PL in the range 15 T 250 K for 0 x 1.0 [328]. (f) CdHgSe CdxHg1xSe crystallizes in the zinc-blende structure at 0 < x < 0.77 and in the wurtzite structure at x > 0.81, while a mixed phase of both structures is observed at 0.77 < x < 0.81 [329]. The composition dependence of E0 for CdxHg1xSe is shown in Figure 6.56(f). The experimental data in the zinc-blende region are taken from Summers and Broerman [330] (solid circle), and those in the wurtzite region are taken from Himei and Muto [331] (open circles) and Pujari et al. [332] (open triangles). The E0 versus x data in the zinc-blende region can be satisfactorily approximated by the linear expression. The corresponding slope dE0/dx is given by 1.57 eV, as listed in Table 6.30. The experimental data in the wurtzite region differ largely among the literature, but clearly show nonlinear dependence on x.

204

PROPERTIES OF SEMICONDUCTOR ALLOYS

The interband CPs in CdxHg1xSe have been determined using reflectance spectroscopy for x up to 0.79 [333] and SE for 0 x 0.30 [334]. The E1 and E1 þ D1 CPs are found to linearly increase with increasing x up to 0.4 [333,334] and show an abrupt increase for x above 0.4 [333]. The temperature dependence of E0 for c-CdxHg1xSe has been studied by Summers and Broerman [330]. These results are shown in Figure 6.57(a). The experimental data suggest that the alloys at x < 0.7 have positive temperature coefficients. The solid line represents the dE0/dT versus x plots obtained from the linear interpolation between the HgSe ( þ 7.4 104 eV/K) and w-CdSe values (3.63 104 eV/K) [1]. It can be seen that the linear interpolation scheme explains the experimental data very well. 10 6 2

0

-2 (a) CdxHg1-xSe

-6 -10 dE0 / dT(10-4 eV/ K)

10 6 2

0

-2 -6

(b) ZnxHg1-xTe

-10 10 6 2

0

-2 -6 -10

(c) CdxHg1-xTe 0

0. 2

0. 4

0. 6

0. 8

1. 0

x

Figure 6.57 Temperature coefficient dE0/dT as a function of x for (a) CdxHg1xSe, (b) ZnxHg1xTe and (c) CdxHg1xTe. The experimental data are taken for (a) from Summers and Broerman [330] (solid circles), for (b) from Toulouse et al. [360] (solid circles) and for (c) from Hansen et al. [372] (solid line). The solid line in (a) represents the linearly interpolated values between the endpoint binary data taken from Adachi [1] (open squares). The solid line in (b) shows the linear least-squares fit of Equation (6.28)

6.5.4 (II, II)–Te Ternary Alloy (a) BeZnTe BexZn1xTe is a promising material for use as a p-type contact layer in various MgZnCdSebased devices. The composition dependence of E0 for c-BexZn1xTe is shown in Figure 6.58(a). The experimental data are taken from various sources [335–338]. The samples used were grown on InP(100) by MBE [335–337] or from the melt using the high-pressure Bridgman

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS 4.5

3.5

4 (b) Mg xZn1-xTe

(a) BexZn1-xTe

205

(c) MgxCd1-xTe

E0,E gX (eV)

4.0 zinc-blende

3.0

3.5

EgX

3.0 2.5

3

2.5 E0

EgX

X

Eg

E0

2

zinc-blende

E0

zinc-blende

E0 (eV)

2.0 2.0 1 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x 2.4 2.5 2.0 (d) Zn xCd1-xTe (e) ZnxHg1-xTe (f) CdxHg1-x Te 2.0 2.2 1.5 1.5

2.0

zinc-blende

zinc-blende

1.0

1.0 1.8

0.5

0.5

1.6

0

0 zinc-blende

semimetallic

semimetallic

1.4 -0.5 -0.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x

Figure 6.58 Energy of the E0 gap versus x for some (II, II)Te ternaries at 300 K: (a) BexZn1xTe, (b) MgxZn1xTe, (b) MgxCd1xTe, (c) ZnxCd1xTe, (d) ZnxHg1xTe and (e) CdxHg1xTe. (f) The solid lines represent the calculated results using the data in Table 6.30. The dashed lines in (a)–(c) show the x dependence of EgX obtained by the linear interpolation between the endpoint binary data in Table 6.1. The gray lines in (d) represent the E0 versus x curves calculated using the experimental c values listed in Table 6.31. The heavy dashed line in (d) shows the E0 versus x curve calculated from the average c value of 0.27 eV

method [338]. These data suggest that the E0 gap is almost linearly dependent upon Be content x. Indeed, the least-squares fit of these data can be described by E0(x) ¼ 2.27 þ 1.83x eV (solid line, see also Table 6.30). The dashed line in Figure 6.58(a) shows the x dependence of EgX for cBexZn1xTe obtained by the linear interpolation between the ZnTe (x ¼ 0) and BeTe values (x ¼ 1.0) in Table 6.1. The G–X crossover is expected to occur at x 0.35 (E0 ¼ EgX 2.9 eV) for c-BexZn1xTe. The composition dependence of the higher-lying CPs, E0 þ D0, E1, E1 þ D1 and E2, for cBexZn1xTe has been determined using SE [336,337]. The E0 þ D0, E1 and E1 þ D1 CP energies increase at a rate of 0.8x eV, while E2 is found to increase at a lower rate of 0.2x eV. It is interesting to note the absence of bowing in any of the CPs. This is in contrast to most of the II–VI ternary alloys, such as BexZn1xSe [303] and ZnxCd1xSe [324], which all exhibit some degree of bowing about the CP energies. (b) MgZnTe MgxZn1xTecrystallizesinthezinc-blendestructureat0 x 0.53andinthewurtzitestructureat x 0.53 [339]. The E0 versus x data for c-MgxZn1xTe determined by wavelength-modulation

206

PROPERTIES OF SEMICONDUCTOR ALLOYS

(open circles) [340] and optical absorption spectroscopy (solid circle) are shown in Figure 6.58 (b) [341]. All samples used were grown by the Bridgman method. The solid line in Figure 6.58(b) shows the quadratic least-squares fit of these and c-MgTe (x ¼ 1.0) data, providing a value of c 0.46 eV. The dashed line in Figure 6.58(b) shows the x dependence of EgX for c-MgxZn1xTe obtained by the linear interpolation between ZnTe (x ¼ 0) and MgTe (x ¼ 1.0) as shown in Table 6.1. This result predicts the G–X crossover to occur at x 0.5 (E0 ¼ EgX 2.75 eV) for c-MgxZn1xTe. The higher-lying CPs in c-MgxZn1xTe have been studied using SE by Franz et al. [342]. The samples were grown by MBE on GaAs(100) substrates (0 x 0.52). The experimental data obtained by these authors show that the E1 and E1 þ D1 CPs increase almost linearly with increasing x, while a clear decrease in E2 is observed from x ¼ 0 (5.25 eV) to 0.52 (5.0 eV). The temperature variation of E0 for c-MgxZn1xTe has been measured by Barbier et al. [340] and Chung et al. [341]. The dE0/dT values near 300 K are given as (4.5 0.3) 104 (0 x 0.41) [340] and (5.9 0.2) 104 (0 x 0.48) eV/K [341], respectively, and are nearly independent of x. (c) MgCdTe Bulk MgxCd1xTe alloy crystallizes in the zinc-blende structure at 0 x 0.6 and in the wurtzite structure at x 0.75 [343]. The E0 versus x data for c-MgxCd1xTe are plotted in Figure 6.58(c) [344–346]. The samples were grown by the Bridgman method [345] or by MBE on ZnCdTe [344] and GaAs substrates [346]. The solid line represents the quadratic leastsquares fit of these and the c-MgTe (x ¼ 1.0) data. This fit results in a bowing of c 0.54 eV. The composition dependence of EgX for c-MgxCd1xTe obtained from the linear interpolation scheme between CdTe (x ¼ 0) and MgTe (x ¼ 1.0) in Table 6.1 is shown in Figure 6.58(c) by the dashed line. It can be seen that the G–X crossover occurs at x 0.7 with E0 ¼ EgX 2.8 eV, in good agreement with the theoretical prediction by Freytag [347]. The higher-lying CPs in c-MgxCd1xTe have been measured using SE by Choi et al. [345] at 0 x 0.5 and by Ihn et al. [346] at 0 x 0.43. These studies observed the E0 þ D0, E1, E1 þ D1, E2 and E10 CPs. Some CPs, E0 þ D0, E1 and E1 þ D1, increased almost linearly at a rate of (0.7 1.3)x eV, while E2 and E10 showed little dependence on x. (d) ZnCdTe ZnxCd1xTe crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. The dependence of E0 on x for ZnxCd1xTe has been determined by many authors. An overview of the bowing parameter c determined at 300 K is summarized in Table 6.31 and in Figure 6.58(d). The c values in Table 6.31 vary from 0 to 0.48 eV. The average c value is 0.27 eV. The corresponding E0 versus x plots are shown in Figure 6.58(d) by the heavy dashed line (see also Table 6.30). The higher-lying CPs, such as E1, E1 þ D1 and E2, in ZnxCd1xTe have been studied by many authors. These CPs showed no or a very weak nonlinearity with respect to x [348–354]. Several studies, however, reported a clear nonlinearity with respect to x [355,356]. The temperature dependence of E0 for ZnxCd1xTe has been studied using PR [357,358], reflectivity and PL [359]. The Varshni parameters have been determined as a ¼ (4.7 0.1) 104 eV/K and b ¼ 166.5 6.5 K for 0 x 0.3 [357] and a ¼ (4.7 0.2) 104 eV/K and

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

207

Table 6.31 Bowing parameter c for E0 of ZnxCd1xTe determined at 300 K. R ¼ reflectance; ER ¼ Electroreflectance; PL ¼ photoluminescence; OA ¼ optical absorption; PR ¼ photoreflectance; SE ¼ spectroscopic ellipsometry c (eV)

Method

Reference

0.33 0.26 0 0.139 0.22890 0.38 0.11 0.128 0.46 0.269 0.48 0.3156 0.334 0.33 0.197 0.33

R ER R PL OA OA PL PR OA SE OA OA PR R SE PR

a b c d e f g h i j k l m n o p

A. Ebina et al., J. Appl. Phys. 44, 3659 (1973) V. A. Tyagai et al., Sov. Phys. Solid State16, 885 (1974) c V. V. Sobolev et al., Phys. Status Solidi B 103, 499 (1981) d D. J. Olego et al., Appl. Phys. Lett. 47, 1172 (1985) e S. M. Johnson et al., J. Vac. Sci. Technol. B 9, 1897 (1991) f A. Aydinli et al., Solid State Commun. 80, 465 (1991) g H. C. Poon et al., J. Phys.: Condens. Matter 7, 2783 (1995) h S. P. Tobin et al., J. Electron. Mater. 24, 697 (1995) i B. Samanta et al., Vacuum 46, 739 (1995) j O. Castaing et al., J. Phys.: Condens. Matter 8, 5757 (1996) k D. Ohlmann et al., J. Appl. Phys. 82, 1355 (1997) l J. Franc et al., Semicond. Sci. Technol. 15, 561 (2000) m L. Tirado-Mejıa et al., Phys. Status Solidi B 220, 255 (2000) n E. M. Larramendi et al., Semicond. Sci. Technol. 17, 8 (2002) o P. D. Paulson et al., J. Appl. Phys. 95, 3010 (2004) p O. Zelaya-Angel et al., J. Appl. Phys. 95, 6284 (2004) a b

b ¼ 110 30 K for 0.551 x 0.944[359].These parameters provide dE0/dT 4 104 eV/ K near 300 K. The corresponding endpoint data are 4.53 104 eV/K (ZnTe) and 3.5 104 eV/K (CdTe) [1]. (e) ZnHgTe ZnxHg1xTe crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. The E0 versus x data for ZnxHg1xTe determined by means of optical absorption [360,361] and SE [361,362] are shown in Figure 6.58(e). The samples used were grown by the THM [360,362,363] or from interdiffusion between the endpoint materials at high temperatures [361]. The quadratic least-squares fit of these data is shown in Figure 6.58(e)

208

PROPERTIES OF SEMICONDUCTOR ALLOYS

by the solid line. The bowing parameter of c 0.46 eV can be determined from this fit (see also Table 6.30). The semimetallic region is in the range x < 0.08 at 300 K. The higher-lying CPs, E0 þ D0, E1, E1 þ D1 and E2, as a function of x for ZnxHg1xTe have been determined using SE [363]. The bowing parameters obtained are c ¼ 0.860 eV (E0 þ D0), 1.012 eV (E1), 0.817 eV (E1 þ D1) and 0.428 eV (E2). The temperature dependence of E0 for ZnxHg1xTe has been investigated by Toulouse et al. [360]. The results obtained are plotted in Figure 6.57(b). It can be seen that the alloy at x < 0.45 has a positive temperature coefficient. The solid line shows the linear least-squares fit given by (in 104 eV/K) dE0 ¼ 4:510:6x dT

ð6:28Þ

(f) CdHgTe CdxHg1xTe crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. Figure 6.58(f) plots the experimental E0 versus x data for CdxHg1xTe measured by Sredin et al. [364] (open circles), Laurenti et al. [365] (solid circles) and Chu et al. [366] (open triangles). The solid line shows the quadratic least-squares fit of these experimental data. The resulting bowing parameter is c 0.21 eV (Table 6.30). The semimetallic region is expected at x < 0.1 and 300 K. The higher-lying CPs, such as E1, E1 þ D1 and E2, as a function of x for CdxHg1xTe have been studied by fundamental reflectivity [364,367], ER [368] and SE [369,370]. They appeared at energies 2–3 (E1), 3–4 (E1 þ D1) and 4.5–5 eV (E2) and gradually increased with increasing x. The bowing parameters determined were c 0.7 0.9 eV for E1 and 0.5 0.6 eV for E1 þ D1 [369]. The c value for E2 was found to be negligibly small (c ¼ 0.06 eV). The temperature dependence of E0 for CdxHg1xTe has been studied by several authors [365,366,371,372]. The result obtained by Hansen et al. [372] is shown in Figure 6.57 (c). The sign for dE0/dT is positive at x < 0.5 and negative at x > 0.5. No temperature change in E0 can be expected at x 0.5 (E0 0.6 eV, Figure 6.58(f)). The dE0/dT value can then be given by (in 104 eV/K) dE0 ¼ 5:511:0x dT

ð6:29Þ

The temperature coefficients of the higher-lying CPs have been measured by several authors [367,373,374]. A dip in the dEg/dT versus x data has been observed near x 0.5 for E1, E1 þ D1, e1 and e1 þ D1 [367]. The E1-gap Varshni parameters a and b have also been determined using ER [373].

6.5.5 Zn–(VI, VI) Ternary Alloy (a) ZnOS ZnOxS1x is one of the II–VI large size-mismatched alloys and may thus behave in a similar manner to GaNx As1x [375]. The E0 gap as a function of x for ZnOxS1x has been determined from transmission measurements by Meyer et al. [376]. The alloy films (0 x 1.0) used were

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

209

grown by rf reactive sputtering on glass and (0001)-sapphire substrates and showed wurtzite structure with preferential c-axis orientation independent of whether glass or sapphire substrates were used. Figure 6.59(a) plots the E0 versus x data measured by Meyer et al. [376]. The solid line shows the quadratic fit of these data and results in a huge bowing parameter of c ¼ 4.50 eV (Table 6.30). This is in qualitative agreement with the fact that bowing parameters in large size-mismatched II–VI alloys increase as the size and chemical mismatches between the endpoint constituents increase [375]. 4.0

4.0 (a) ZnOxS1-x

3.5

4.0 (b) ZnSxSe1-x

3.5

4.0 (c) ZnSxTe1-x

3.5

(d) ZnSexTe1-x

3.5

E0 (eV)

zinc-blende

zinc-blende

3.0

3.0

3.0

3.0

2.5

2.5

2.5

2.5

2.0

2.0

2.0

2.0 wurtzite

zinc-blende

1.5 1.5 1.5 1.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0

x

x

x

x

Figure 6.59 Energy of the E0 gap versus x for some Zn–(VI, VI) ternaries at 300 K: (a) ZnOxS1x, (b) ZnSxSe1x, (c) ZnSxTe1x and (d) ZnSexTe1x. The solid lines represent the calculated results using the data in Table 6.30

(b) ZnOSe ZnOxSe1x at x ¼ 0.35 1.3 at% has been successfully grown on GaAs(100) by MBE in spite of the limited solubility of oxygen in ZnSe [377]. A large bowing parameter, as high as 8 eV has been obtained [377] and a reduced pressure coefficient has been successfully explained within the framework of the BAC model [378]. More recently, the temperature variation of E0 in ZnOxSe1x (x ¼ 0.23 0.90 at%) before and after hydrogen passivation was found to be similar to that for ZnSe and did not depend on the oxygen concentration [379]. Such a finding points toward the absence of a localized character in the ZnOxSe1x band edge. (c) ZnSSe c-ZnSxSe1x can be grown from the melt throughout the whole composition range 0 x 1.0, although the alloy at x 0.9 sometimes shows a short-range twin structure which is typically observed in ZnS grown from the melt [380]. We show in Figure 6.59(b) the x dependence of E0 in ZnSxSe1x determined by fundamental reflectivity [380] (solid circles), CL [381] (open circles) and optical absorption measurements [382] (open triangles). The solid line shows the quadratic least-squares fit of these data. The resulting bowing parameter is c ¼ 0.580 eV (Table 6.30). The low-temperature (T 6 K) E0 versus x data for ZnSxSe1x have also been reported [381,383]. The pressure coefficient dE0/ dp for p up to 12 GPa has been measured by Griebl et al. [382].

210

PROPERTIES OF SEMICONDUCTOR ALLOYS

(d) ZnSTe ZnSxTe1x is one of the II–VI large size-mismatched alloys and may have a large bowing of the E0 gap. The E0 versus x data reported by Hill and Richardson [384] (solid circles), Yu et al. [385] (open circles) and by Walukiewicz et al. [386] (open triangles) are shown in Figure 6.59(c). The samples were grown by vacuum evaporation [384], hot-wall epitaxy [385] or by the Bridgman method [386]. The solid line in Figure 6.59(c) shows the quadratic least-squares fit of the data of Yu et al. and Walukiewicz et al. The resulting bowing parameter is c ¼ 3.750 eV (Table 6.30). The data of Hill and Richardson gave a value of c 3.0 eV [384]. SE has been used by Bang et al. [387] on ZnSxTe1x epilayers (0 x 1.0) grown on GaAs (100) substrates by hot-wall epitaxy. The E0 þ D0 and E1 structures merged into a single, broad structure for x larger than 0.3. The pressure dependence of E0 in ZnSxTe1x (x ¼ 0–0.1) has been studied by Walukiewicz et al. [386] (x ¼ 0–0.1) for p up to 10 GPa. A strong nonlinear dependence of E0 on p was observed by optical absorption measurements. The results can be satisfactorily described by the BAC model. (e) ZnSeTe ZnSexTe1x crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. The composition dependence of E0 has been studied by several authors. The E0 versus x data measured by Larach et al. [388] (solid circles), Ebina et al. [389] (open circles), Brasil et al. [390] (solid triangles) and Su et al. [391] (open triangles) have been plotted in Figure 6.59(d) The quadratic least-squares fit of these data is shown by the solid line. The bowing parameter obtained is c ¼ 1.500 eV (Table 6.30). This value is considerably larger than that for ZnSxSe1x (c ¼ 0.580 eV, Figure 6.59(b)), but is much smaller than those for ZnOxS1x (c ¼ 4.50 eV, Figure 6.59(a)) and ZnSxTe1x (c ¼ 3.750 eV, Figure 6.59(c)). The higher-lying CPs, such as E0 þ D0, E1, E1 þ D1 and E2, as a function of x for ZnSexTe1x have been measured by fundamental reflectivity [389] and SE [392]. The bowing parameters determined were c ¼ 1.878 eV (E1), 1.458 eV (E1 þ D1) and 0.698 eV (E2) [392]. Only the E2 CP gives an upward bowing (c < 0 eV). The high-energy PL line as a function of temperature T for ZnSexTe1x (0 x 0.30) has been measured by Naumov et al. [393]. The experimental data could be fitted with the Varshni expression using the interpolated parameters between ZnTe (x ¼ 0) and ZnSe (x ¼ 1.0) [1]. The pressure dependence of E0 has also been measured for p up to 10 GPa [394]. The first- and second-order pressure coefficients are reported as a function of x for 0 x 1.0. The large deviation of dE0/dp from the linear interpolation can be explained by the BAC model [394].

6.5.6 Cd–(VI, VI) Ternary Alloy (a) CdSSe CdSxSe1x crystallizes in the wurtzite structure over the whole composition range 0 x 1.0. The experimental E0 value as a function of x for w-CdSxSe1x measured by Bondarenko et al. [395] (solid circles) and Perna et al. [396] are shown in Figure 6.60(a). The quadratic fit of these data gives a value of c ¼ 0.700 eV (Table 6.30).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

211

The higher-lying CPs, such as E1, E2 and E10, in w-CdSxSe1x have been determined from the fundamental reflectivity measurements for the ordinary (E ? c) and extraordinary rays (E||c) at 90 K [397]. The temperature dependence of E0 in w-CdSxSe1x has been studied by Perna et al. [396]. These authors reported that the effects of the acoustic phonons are larger in alloy films than in the related binaries because of the compositional disorder. (b) CdSTe The CdS–CdTe phase diagram indicates that at low temperatures, CdSxTe1x has a zinc-blende structure for low S concentrations and a wurtzite structure for high S concentrations (Figure 2.7). These regions are separated by a miscibility gap where both phases exist, and optical transitions resulted from both wide band-gap wurtzite and narrow band-gap zinc-blende phases. Therefore, the two absorption edges would usually be detected, although their strengths would depend on the concentration of each phase. Many authors have measured the E0 versus x data for CdSxTe1x films (see Lane [398]). A small number of samples of different x have been studied generally, with the most widely accepted results relying on 19 data points from x ¼ 0 to 1.0 reported by Ohata et al. [399]. From the quadratic fit of the previous data, we obtain a bowing parameter of c 1.8 eV for both the zinc-blende and wurtzite phases (see also Figure 1 in Lane [398] and Figure 6.63). The curves plotted in Figure 6.60(b) show the quadratic fits of Equation (A.5) with c 1.8 eV (Table 6.30). 3.00

2.6

(a) CdSxSe1-x 2.75

1.8

(b) CdSxTe1-x 2.4

(c) CdSexTe1-x 1.7

miscibility gap

E0 (eV)

2.50

wurtzite

2.2

zinc-blende

1.6 zinc-blende

2.25

2.0

2.00

1.8

wurtzite

1.5 1.4

wurtzite

1.75

1.6

1.3 zinc-blende

1.50

0 0.2 0.4 0.6 0.8 1.0 x

1.4

0 0.2 0.4 0.6 0.8 1.0 x

1.2

0 0.2 0.4 0.6 0.8 1.0 x

Figure 6.60 Energy of the E0 gap versus x for some Cd(VI, VI) ternaries at 300 K: (a) CdSxSe1x, (b) CdSxTe1x and (c) CdSexTe1x. The solid and dashed lines represent the calculated results using the data in Table 6.30

The higher-lying CPs in c-CdSxTe1x (x ¼ 0 1.0) have been determined using SE [400]. The samples used were deposited on borosilicate glass (Corning 7059) using a laser-deposition process. The XRD analysis suggested that the deposited films consisted of a single phase. The bowing parameter determined for the E1 gap is c 0.8 eV, while that for E0 is 1.84 eV. (c) CdSeTe Since CdSe is a wurtzite crystal while CdTe is a zinc-blende crystal, it is reasonable to expect a phase change in crystal structure at some Se composition. This has been reported for alloys

212

PROPERTIES OF SEMICONDUCTOR ALLOYS

grown on glass substrates with zinc-blende nucleation at x < 0.60 and wurtzite nucleation at x > 0.60 [401]. Similarly, melt-grown CdSexTe1x was reported to nucleate as zinc-blende at x 0.45 and as wurtzite at x 0.65 with a mixed phase between x ¼ 0.45 and 0.65 [402]. Figure 6.60(c) shows the plots of E0 against x for c-CdSexTe1x reported by Feng et al. [403] (solid circles) and Brill et al. [404] (open circles). The samples were grown by the Bridgman method (x < 0.36) [403] and by MBE on Si(211) (0 x 1.0) [404]. It could be clearly observed that the MBE-grown CdSexTe1x/Si(211) films remained in the cubic phase throughout the entire composition range [404]. Note that CdSe can be grown in the cubic phase on GaAs and ZnSe substrates (see Brill et al. [404]). The solid line in Figure 6.60(c) represents the quadratic least-squares fit of the experimental data, yielding a value of c ¼ 0.838 eV (Table 6.30).

6.5.7 (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe MgxZn1xSySe1y can be grown lattice-matched to GaAs (Table 1.13) and has been used as an improved cladding material for ZnSe-based waveguiding devices [405]. The E0-gap energy as a function of x for MgxZn1xSySe1y/GaAs calculated from Equation (A.15) is shown in Figure 6.61(a).The experimental data shown are taken from Lunz et al. [406]

5.0

4.0

5.0

3.5

(a) MgxZn1-xSySe1-y /GaAs 4.5

3.0

4.5

2.5 2.0 0

4.0 E0 (eV)

E0 (eV)

4.0 3.5

on ZnTe

0.5

1.0

3.5

3.0

3.0

2.5

2.5

2.0

2.0

(b) MgxZn1-xSeyTe1-y /InP 0

0.2

0.4

0.6 x

0.8

1.0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.61 Energy of the E0 gap versus x for (a) MgxZn1xSySe1y/GaAs and (b) MgxZn1x

SeyTe1y/InP calculated from Equation (A.15). The ternary bowing parameters are taken from Table 6.32. The unknown ternary and quaternary bowing parameters (c and D) are assigned to be 0 eV. The experimental data in (a) are taken from Lunz et al. [406] (solid circles) and Chen et al. [407] (open circle) and in (b) from Naniwae et al. [408] (300 K). The dashed line in (a) shows the quadratic approximation of Equation (A.15) for 0 x 0.5 (see Table 6.30). The inset in (b) represents the E0 versus x data for MBE-grown MgxZn1xSeyTe1y/ZnTe reported by Shim et al. [409]. The solid line in the inset is calculated from Equation (6.30)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

213

(solid circles) and Chen et al. [407] (open circle). It can be seen that the calculated E0 varies from 2.749 eV (x ¼ 0, y ¼ 0.06) to 4.399 eV (x ¼ 1.00, y ¼ 0.89). This curve can be approximated by the quadratic expression as shown in Figure 6.61(a) by the dashed line (Table 6.30). The temperature dependence of E0 for MgxZn1xSySe1y/GaAs has been determined by Lunz et al. [406] from an optical absorption and by Chen et al. [407] from contactless ER. The dE0/dT coefficient near 300 K is 6 104 eV/K, while that for ZnSe is 4.7 104 eV/ K [1]. (b) MgZnSeTe MgxZn1xSeyTe1y can be grown lattice-matched to InP (Table 1.13). The solid line in Figure 6.61(b) shows the E0 versus x curve for MgxZn1xSeyTe1y/InP obtained from Equation (A.15). The solid circles represent the experimental data measured by optical reflectivity [408]. The solid line can be approximated by the quadratic expression given in Table 6.30. MgxZn1xSeyTe1y can be grown lattice-matched to ZnTe. Shim et al. [409] grew MgxZn1xSeyTe1y/ZnTe by MBE and determined E0 from PL measurements. The inset in Figure 6.61(b) shows the E0 versus x data of Shim et al. [409]. These data can be least-squares fit as (in eV) E0 ðxÞ ¼ 2:36 þ 0:89x þ 0:82x2

ð6:30Þ

6.5.8 (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe BexMgyZn1xySe can be grown lattice-matched to GaAs (Table 1.14). The experimental E0 versus y data for BexMgyZn1xySe/GaAs are plotted in Figure 6.62(a). These data are taken from Wagner et al. [410] (solid circles) and Godo et al. [411] (open circles). The solid line represents the E0 versus y curve for BexMgyZn1xySe/GaAs calculated from Equation (A.15). This curve can be satisfactorily approximated by the quadratic expression shown in Table 6.30. The E0/(E0 þ D0) structure of Bridgman-grown BexMgyZn1xySe alloy (x ¼ 0.04, y ¼ 0.15) has been investigated by PL, contactless ER and PR in the temperature range between 15 and 400 K [412]. The obtained data were analyzed using the Varshni and Bose–Einstein expressions. (b) BeZnCdSe Bulk BexZnyCd1xySe alloys were grown by the Bridgman method and investigated using ER, PR, SE and PL [413–415]. The samples were single wurtzite phase or wurtzite as the main phase in an admixture with another polytype (x 0.15, y 0.45). The temperature dependence of E0 has been reported [413,415]. BexZnyCd1xySe can be epitaxially grown lattice-matched to InP. Hsieh et al. [416] have characterized the E0 structure of MBE-grown BexZnyCd1xySe/InP using contactless ER and PzR in the temperature range between 15 and 450 K. The results show that Be incorporation can effectively reduce the rate of temperature variation of E0.

214

PROPERTIES OF SEMICONDUCTOR ALLOYS 5.0

4.0

(a) Bex Mgy Zn1-x-y Se/GaAs

(b) Mg x Zny Cd 1-x-y Se/InP

4.5 3.5 E0 (eV)

E0 (eV)

4.0 3.5

3.0

3.0 2.5 2.5 2.0

0

0.2

0.4

0.6

0.8

1.0

2.0

0

0.2

y

0.4

0.6

0.8

1.0

x

Figure 6.62 Energy of the E0 gap versus y or x for (a) BexMgyZn1xySe/GaAs and (b)

MgxZnyCd1xySe/InP calculated from Equation (A.15). The ternary bowing parameters are taken from Table 6.32 (see also Table 6.30). The unknown ternary and quaternary bowing parameters (c and D) are assigned to be 0 eV. The experimental data in (a) are taken from Wagner et al. [410] (solid circles) and Godo et al. [411] (open circles) (300 K). The solid circles in (b) are obtained from Maksimov et al. [417]. The solid lines show the quadratic approximations listed in Table 6.30 (c) MgZnCdSe MgxZnyCd1xySe can be grown, together with those for the E0 and E0 þ D0 CPs latticematched to InP (Table 1.14). Figure 6.62(b) plots the E0 versus x data for MgxZnyCd1xySe/ InP measured by Maksimov et al. [417]. The E0 versus x curve calculated from Equation (A.15) is shown by the solid line. The corresponding quadratic expression is given in Table 6.30. The temperature dependence of E0 has also been determined by Maksimov et al. [417] in the temperature range between 4.2 and 300 K.

6.5.9 Summary Table 6.32 summarizes the bowing parameter c for E0 in some II–VI ternary alloys. Figure 6.63 also shows the plots for the c value against the product DaabDXab of the lattice constant and electronegativity differences between the endpoint binaries a and b. The electronegativity differences are obtained from Phillips [46]. The solid line in Figure 6.63 represents the leastsquares fit obtained using the relationship (c in eV, DaabDXab in AeV) c ¼ 6:13ðDaab DXab Þ

ð6:31Þ

Note that the proportionality factor 6.13 A1 obtained here is considerably smaller than the 1 values 9.93 and 9.62 A for the group-IV binary and III–V ternary alloys, respectively (Equations (6.8) and (6.23)). Finally, the relationships between the E0 gap and lattice constant a0 for various II–VI semiconductors are shown in Figure 6.64. It is clear that the lowest direct gap E0 can be widely

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

215

Table 6.32 Bowing parameter c for E0 in II–VI ternaries. w ¼ wurtzite; zb ¼ zinc-blende (II, II)–VI

c (eV)

II–(VI, VI)

c (eV)

BeZnO (w) MgZnO (w) ZnCdO (w) MgZnS (zb) MgZnS (w) ZnCdS (zb) ZnCdS (w) ZnHgS (zb) CdHgS (w) BeZnSe (zb) BeCdSe (zb) MgZnSe (zb) MgCdSe (zb) MgCdSe (w) ZnCdSe (zb) CdHgSe (zb) BeZnTe (zb) MgZnTe (zb) MgCdTe (zb) ZnCdTe (zb) ZnHgTe (zb) CdHgTe (zb)

9.3 0 2.4 0 0 0.827 0.921 0.996 0 1.033 3.000 0.600 0.200 0 0.387 0 0 0.46 0.54 0.31 0.46 0.21

ZnOS (w) ZnSSe (zb) ZnSTe (zb) ZnSeTe (zb) CdSSe (w) CdSTe (zb) CdSTe (w) CdSeTe (zb)

4.50 0.580 3.750 1.500 0.700 1.80 1.800 0.838

6.0 5.0

c (eV)

4.0

ZST BCSe

3.0 CST

2.0

ZSeT ZHS

1.0

BZSe CSeT

0

0

0.20

0.40

0.60

0.80

1.00

∆aAB∆XAB (Å eV)

Figure 6.63 Bowing parameter c of the E0 gap versus product DaabDXab of the lattice-constant and electronegativity differences between the endpoint binary materials a and b in some II–VI semiconductor ternary alloys. The solid line represents the calculated result using Equation (6.31). B ¼ Be; Z ¼ Zn; C ¼ Cd; T ¼ Te

216

PROPERTIES OF SEMICONDUCTOR ALLOYS GaP GaAs

6

InP

InAs

InSb

BeSe 5

MgS BeTe

4

ZnS

MgTe

ZnSe

3

E0 (eV)

MgSe

CdS

ZnTe

2

CdSe

CdTe

1 0

HgS

Semimetallic -1 5.0

5.2

5.4

5.6

5.8

6.0

HgSe 6.2

HgTe 6.4

6.6

6.8

a (Å)

Figure 6.64 Relationships between the E0 gap and lattice constant a0 for II–VI semiconductor systems

varied by properly combining the binary materials when growing II–VI ternary and quaternary alloys. Such alloys can be epitaxially grown on commercially available III–V binary substrates, such as GaP, GaAs and InP.

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] J. L. Birman, Phys. Rev. 115, 1493 (1959). [3] D. G. Thomas and J. J. Hopfield Phys. Rev. 116, 573 (1959); J. J. Hopfield J. Phys. Chem. Solids 15, 97 (1960). [4] J. A. Van Vechten and T. K. Bergstresser, Phys. Rev. B 1, 3351 (1970). [5] J. C. Phillips and J. A. Van Vechten, Phys. Rev. Lett. 22, 705 (1969). [6] P. Kiesel, T. Kippenberg, and G. H. D€ohler, in Spontaneous Ordering in Semiconductor Alloys (edited by A. Mascarenhas), Kluwer Academic, New York, 2002, p. 365. [7] G. F. Koster, J. O. Dimmock, R. G. Wheeler, and H. Statz, Properties of Thirty-Two Point Groups, MIT Press, Cambridge, 1963. [8] P. Ernst, C. Geng, F. Scholz, H. Schweizer, Y. Zhang, and A. Mascarenhas, Appl. Phys. Lett. 67, 2347 (1995). [9] B. T. McDermott, K. G. Reid, N. A. El-Masry, S. M. Bedair, W. M. Duncan, X. Yin, and F. H. Pollak, Appl. Phys. Lett. 56, 1172 (1990). [10] R. L. Forrest, T. D. Golding, S. C. Moss, Z. Zhang, J. F. Geisz, J. M. Olson, A. Mascarenhas, P. Ernst, and C. Geng, Phys. Rev. B 58, 15355 (1998). [11] W. Kissinger, M. Weidner, H. J. Osten, and M. Eichler, Appl. Phys. Lett. 65, 3356 (1994). [12] S. Zollner, C. M. Herzinger, J. A. Woollam, S. S. Iyer, A. P. Powell, and K. Eberl, Solid State Commun. 96, 305 (1995). [13] A. A. Demkov and O. F. Sankey, Phys. Rev. B 48, 2207 (1993).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

217

[14] H. Lee, S. R. Kurtz, J. A. Floro, J. Strane, C. H. Seager, S. R. Lee, E. D. Jones, J. F. Nelson, T. Mayer, and S. T. Picraux, Jpn. J. Appl. Phys. 34, L1340 (1995). [15] S. Zollner, K. E. Junge, R. Lange, and A. A. Affolder, Jpn. J. Appl. Phys. 35, 5684 (1996). [16] J. Kolodzey, P. A. O’Neil, S. Zhang, B. A. Orner, K. Roe, K. M. Unruh, C. P. Swann, M. M. Waite, and S. I. Shah, Appl. Phys. Lett. 67, 1865 (1995). [17] J. S. Schrader, J. L. Huguenin-Love, R. J. Soukup, N. J. Ianno, C. L. Exstrom, S. A. Darveau, R. N. Udey, and V. L. Dalal, Sol. Ener. Mater. Sol. Cells 90, 2338 (2006). [18] K. E. Junge, N. R. Voss, R. Lange, J. M. Dolan, S. Zollner, M. Dashiell, D. A. Hits, B. A. Orner, R. Jonczyk, and J. Kolodzey, Thin Solid Films 313–314, 172 (1998). [19] See, for example, Semiconductors and Semimetals (edited by R. K. Willardson and A. C. Beer), Academic, New York, 1991, Vol. 33 (Volume Editor, T. P. Pearsall). [20] R. Braunstein, A. R. Moore, and F. Herman, Phys. Rev. 109, 695 (1958). [21] J. Weber and M. I. Alonso, Phys. Rev. B 40, 5683 (1989). [22] D. V. Lang, R. People, J. C. Bean, and A. M. Sergent, Appl. Phys. Lett. 47, 1333 (1985). [23] D. Dutartre, G. Bremond, A. Souifi, and T. Benyattou, Phys. Rev. B 44, 11525 (1991). [24] C. W. Liu, J. C. Sturm, Y. R. J. Lacroix, M. L. W. Thewalt, and D. D. Perovic, Appl. Phys. Lett. 65, 76 (1994). [25] R. People, Phys. Rev. B 32, 1405 (1985); 34, 2508 (1986). [26] F. Ferrieu, F. Beck, and D. Dutartre, Solid State Commun. 82, 427 (1992). [27] R. T. Carline, C. Pickering, D. J. Robbins, W. Y. Leong, A. D. Pitt, and A. G. Cullis, Appl. Phys. Lett. 64, 1114 (1994). [28] R. T. Carline, T. J. C. Hosea, and D. J. Hall, J. Appl. Phys. 78, 4285 (1995). [29] J. H. Bahng, K. J. Kim, S. H. Ihm, and J. Y. Kim, Solid State Commun. 106, 591 (1998). [30] T. Ebner, K. Thonke, R. Sauer, F. Schaeffler, and H. J. Herzog, Phys. Rev. B 57, 15448 (1998). [31] P. Etchegoin, J. Kircher, and M. Cardona, Phys. Rev. B 47, 10292 (1993). [32] J. Humlıcek, F. Lukes, E. Schmidt, M. G. Kekoua, and E. Khoutsishvili, Phys. Rev. B 33, 1092 (1986). [33] E. Schmidt and K. Vedam, Solid State Commun. 9, 1187 (1971). [34] G. He and H. A. Atwater, Phys. Rev. Lett. 79, 1937 (1997). [35] H. P. L. de Guevara, A. G. Rodrıguez, H. Navarro-Contreras, and M. A. Vidal, Appl. Phys. Lett. 84, 4532 (2004); 91, 161909 (2007). [36] M. R. Bauer, J. Tolle, C. Bungay, A. V. G. Chizmeshya, D. J. Smith, J. Menendez, and J. Kouvetakis, Solid State Commun. 127, 355 (2003). [37] V. R. D’Costa, C. S. Cook, A. G. Birdwell, C. L. Littler, M. Canonico, S. Zollner, J. Kouvetakis, and J. Menendez, Phys. Rev. B 73, 125207 (2006). [38] A. S. Amour, C. W. Liu, J. C. Sturm, Y. Lacroix, and M. L. W. Thewalt, Appl. Phys. Lett. 67, 3915 (1995). [39] C. G. Van de Walle and R. M. Martin, Phys. Rev. B 34, 5621 (1986). [40] O. G. Schmidt and K. Eberl, Phys. Rev. Lett. 80, 3396 (1998). [41] H. Lee, J. A. Floro, J. Strane, S. R. Lee, E. D. Jones, T. Mayer, and S. T. Picraux, Mater. Res. Soc. Symp. Proc. 379, 211 (1995). [42] W. Kissinger, H. J. Osten, M. Weidner, and M. Eichler, J. Appl. Phys. 79, 3016 (1996). [43] P. Aella, C. Cook, J. Tolle, S. Zollner, A. V. G. Chizmeshya, and J. Kouvetakis, Appl. Phys. Lett. 84, 888 (2004). [44] V. R. D’Costa, C. S. Cook, J. Menendez, J. Tolle, J. Kouvetakis, and S. Zollner, Solid State Commun. 138, 309 (2006). [45] R. A. Soref, J. Appl. Phys. 70, 2470 (1991). [46] J. C. Phillips, Bonds and Bands in Semiconductors, Academic, New York, 1973. [47] H. Okumura, T. Koizumi, Y. Ishida, H. Yaguchi, and S. Yoshida, Phys. Status Solidi B 216, 211 (1999). [48] T. Suzuki, H. Yaguchi, H. Okumura, Y. Ishida, and S. Yoshida, Jpn. J. Appl. Phys. 39, L497 (2000).

218

PROPERTIES OF SEMICONDUCTOR ALLOYS

[49] A. Kasic, M. Schubert, T. Frey, U. K€ohler, D. J. As, and C. M. Herzinger, Phys. Rev. B 65, 184302 (2002). [50] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [51] M. P. Thompson, G. W. Auner, T. S. Zheleva, K. A. Jones, S. J. Simko, and J. N. Hilfiker, J. Appl. Phys. 89, 3331 (2001). [52] D. Brunner, H. Angerer, E. Bustarret, F. Freudenberg, R. H€ opler, R. Dimitrov, O. Ambacher, and M. Stutzmann, J. Appl. Phys. Lett. 82, 5090 (1997). [53] J. F. Muth, J. D. Brown, M. A. L. Johnson, Z. Yu, R. M. Kolbas, J. W. Cook, Jr., and J. F. Schetzina, Mater. Res. Soc. Symp. Proc. 537, G5.2 (1999). [54] B. K. Meyer, G. Steude, A. G€oldner, A. Hoffmann, H. Amano, and I. Akasaki, Phys. Status Solidi B 216, 187 (1999). [55] C. Buchheim, R. Goldhahn, M. Rakel, C. Cobet, N. Esser, U. Rossow, D. Fuhrmann, and A. Hangleiter, Phys. Status Solidi B 242, 2610 (2005). [56] I. Vurgaftman and J. R. Meyer, J. Appl. Phys. 94, 3675 (2003). [57] J. Wu, W. Walukiewicz, K. M. Yu, J. W. Ager III, S. X. Li, E. E. Haller, H. Lu, and W. J. Schaff, Solid State Commun. 127, 411 (2003). [58] S. R. Lee, A. F. Wright, M. H. Crawford, G. A. Petersen, J. Han, and R. M. Biefeld, Appl. Phys. Lett. 74, 3344 (1999). [59] T. Wethkamp, K. Wilmers, N. Esser, W. Richter, O. Ambacher, H. Angerer, G. Jungk, R. L. Johnson, and M. Cardona, Thin Solid Films 313–314, 745 (1998). [60] W. Shan, J. W. Ager III, W. Walukiewicz, E. E. Haller, B. D. Little, J. J. Song, M. Schurman, Z. C. Feng, R. A. Stall, and B. Goldenberg, Appl. Phys. Lett. 72, 2274 (1998). [61] F. Yun, M. A. Reshchikov, L. He, T. King, and H. Morko˛c , J. Appl. Phys. 92, 4837 (2002). [62] L. Malikova, Y. S. Huang, F. H. Pollak, Z. C. Feng, M. Schurman, and R. A. Stall, Solid State Commun. 103, 273 (1997). [63] N. Nepal, J. Li, M. L. Nakarmi, J. Y. Lin, and H. X. Jiang, Appl. Phys. Lett. 87, 242104 (2005). [64] W. Shan, J. W. Ager III, K. M. Yu, W. Walukiewicz, E. E. Haller, M. C. Martin, W. R. McKinney, and W. Yang, J. Appl. Phys. 85, 8505 (1999). [65] J. Wu and W. Walukiewicz, Superlatt. Microstruct. 34, 63 (2003). [66] M. Androulidaki, N. T. Pelekanos, K. Tsagaraki, E. Dimakis, E. Iliopoulos, A. Adikimenakis, E. Bellet-Amalric, D. Jalabert, and A. Georgakilas, Phys. Status Solidi C 3, 1866 (2006). [67] W. Terashima, S.-B. Che, Y. Ishitani, and A. Yoshikawa, Jpn. J. Appl. Phys. 45, L539 (2006). [68] R. Goldhahn, P. Schley, A. T. Winzer, G. Gobsch, V. Cimalla, O. Ambacher, M. Rakel, C. Cobet, N. Esser, H. Lu, and W. J. Schaff, Phys. Status Solidi A 203, 42 (2006). [69] S. X. Li, J. Wu, E. E. Haller, W. Walukiewicz, W. Shan, H. Lu, and W. J. Schaff, Appl. Phys. Lett. 83, 4963 (2003). [70] J. Sch€ormann, D. J. As, K. Lischka, P. Schley, R. Goldhahn, S. F. Li, W. L€ offler, M. Hetterich, and H. Kalt, Appl. Phys.Lett. 89, 261903 (2006). [71] J. R. M€ullh€auser, O. Brandt, A. Trampert, B. Jenichen, and K. H. Ploog, Appl. Phys. Lett. 73, 1230 (1998). [72] R. Goldhahn, J. Scheiner, S. Schokhovets, T. Frey, U. K€ ohler, D. J. As, and K. Lischka, Appl. Phys. Lett. 76, 291 (2000). [73] C. A. Parker, J. C. Roberts, S. M. Bedair, M. J. Reed, S. X. Liu, N. A. El-Masry, and L. H. Robins, Appl. Phys. Lett. 75, 2566 (1999). [74] C. Caetano, L. K. Teles, M. Marques, A. Dal Pino, Jr., and L. G. Ferreira, Phys. Rev. B 74, 045215 (2006). [75] P. Schley, R. Goldhahn, A. T. Winzer, G. Gobsch, V. Cimalla, O. Ambacher, H. Lu, W. J. Schaff, M. Kurouchi, Y. Nanishi, M. Rakel, C. Cobet, and N. Esser, Phys. Rev. B 75, 205204 (2007). [76] K. M. Yu, Z. Liliental-Weber, W. Walukiewicz, W. Shan, J. W. Ager III, S. S. Li, R. E. Jones, E. E. Haller, H. Lu, and W. J. Schaff, Appl. Phys. Lett. 86, 071910 (2005).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

219

[77] W. Shan, B. D. Little, J. J. Song, Z. C. Feng, M. Schurman, and R. A. Stall, Appl. Phys. Lett. 69, 3315 (1996). [78] W. Shan, W. Walukiewicz, E. E. Haller, B. D. Little, J. J. Song, M. D. McCluskey, N. M. Johnson, Z. C. Feng, M. Schurman, and R. A. Stall, J. Appl. Phys. 84, 4452 (1998). [79] H. Sonomura, T. Nanmori, and T. Miyauchi, Appl. Phys. Lett. 24, 77 (1974). [80] A. Onton, M. R. Lorenz, J. M. Woodall, and R. J. Chicotka, J. Cryst. Growth 27, 166 (1974). [81] L. K. Vodop’yanov, V. I. Kozlovskiı, and N. N. Mel’nik, Sov. Phys. Semicond. 34, 405 (2000). [82] J. M. Rodrıguez and G. Armelles, J. Appl. Phys. 69, 965 (1991). [83] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, D. H. Woo, and S. H. Kim, J. Appl. Phys. 87, 1287 (2000). [84] A. Onton and R. J. Chicotka, J. Appl. Phys. 41, 4205 (1970). [85] D. P. Bour, J. R. Shealy, G. W. Wicks, and W. J. Schaff, Appl. Phys. Lett. 50, 615 (1987). [86] Y. Ishitani, H. Hamada, S. Minagawa, H. Yaguchi, and Y. Shiraki, Jpn. J. Appl. Phys. 36, 6607 (1997). [87] A. Onton, M. R. Lorenz, and W. Reuter, J. Appl. Phys. 42, 3420 (1971). [88] C. Alibert, G. Bordure, A. Laugier, and J. Chevallier, Phys. Rev. B 6, 1301 (1972). [89] I. Vurgaftman, J. R. Meyer, and L. R. Ram-Mohan, J. Appl. Phys. 89, 5815 (2001). [90] H. Lange, J. Donecker, and H. Friedrich, Phys. Status Solidi B 73, 633 (1976). [91] M. Bugajski, A. M. Kontkiewicz, and H. Mariette, Phys. Rev. B 28, 7105 (1983). [92] R. Hill, J. Phys. C: Solid State Phys. 7, 516 (1974). [93] H. Lee, D. Biswas, M. V. Klein, H. Morko˛c , D. E. Aspnes, B. D. Choe, J. Kim, and C. O. Griffiths, J. Appl. Phys. 75, 5040 (1994). [94] Y. Ishitani, H. Yaguchi, and Y. Shiraki, Jpn. J. Appl. Phys. 40, 1183 (2001). [95] Y. C. Yeh, S. Chen, Y. S. Huang, C. H. Ho, and K. K. Tiong, J. Phys.: Condens. Matter 12, 2183 (2000). [96] R. Ferrini, G. Guizzetti, M. Patrini, A. Parisini, L. Tarricone, and B. Valenti, Eur. Phys. J. B 27, 449 (2002). [97] A. Onton and R. J. Chicotka, Phys. Rev. B 4, 1847 (1971). [98] B. W. Hakki, A. Jayaraman, and C. K. Kim, J. Appl. Phys. 41, 5291 (1970). [99] A. R. Go~ni, K. Syassen, K. Str€ossner, and M. Cardona, Phys. Rev. B 39, 3178 (1989). [100] J. Chen, D. Patel, J. R. Sites, I. L. Spain, M. J. Hafich, and G. Y. Robinson, Solid State Commun. 75, 693 (1990). [101] J. Dong, G. Li, Z. Wang, D. Lu, X. Liu, X. Li, D. Sun, M. Kong, and Z. Wang, J. Appl. Phys. 79, 7177 (1996). [102] J. L. Aubel, U. K. Reddy, S. Sundaram, W. T. Beard, and J. Comas, J. Appl. Phys. 58, 495 (1985). [103] D. E. Aspnes, S. M. Kelso, R. A. Logan, and R. Bhat, J. Appl. Phys. 60, 754 (1986). [104] A. K. Saxena, Phys. Status Solidi B 105, 777 (1981). [105] B. Monemar, K. K. Shih, and G. D. Pettit, J. Appl. Phys. 47, 2604 (1976). [106] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [107] H. J. Lee, L. Y. Juravel, J. C. Woolley, and A. J. Spring Thorpe, Phys. Rev. B 21, 659 (1980). [108] J. C. M. Henning, J. P. M. Ansems, and P. J. Roksnoer, J. Phys. C: Solid State Phys. 19, L335 (1986). [109] B. Wakefield, M. A. G. Halliwell, T. Kerr, D. A. Andrews, G. J. Davies, and D. R. Wood, Appl. Phys. Lett. 44, 341 (1984). [110] W. Y. Chou, G. S. Chang, W. C. Hwang, and J. S. Hwang, J. Appl. Phys. 83, 3690 (1998). [111] D. Oertel, D. Bimberg, R. K. Bauer, and K. W. Carey, Appl. Phys. Lett. 55, 140 (1989). [112] A. Convertino, G. Padeletti, L. Cerri, and S. Viticoli, J. Vac. Sci. Technol. B 20, 243 (2002). [113] R. E. Nahory, M. A. Pollack, and J. C. DeWinter, J. Appl. Phys. 46, 775 (1975). [114] T. J. Kim, T. H. Ghong, Y. D. Kim, S. J. Kim, D. E. Aspnes, T. Mori, T. Yao, and B. H. Koo, Phys. Rev. B 68, 115323 (2003). [115] D. K. Gaskill, N. Bottka, L. Aina, and M. Mattingly, Appl. Phys. Lett. 56, 1269 (1990).

220

PROPERTIES OF SEMICONDUCTOR ALLOYS

[116] J. Singh, in Properties of Lattice-matched and Strained Indium Gallium Arsenide, EMIS Datareviews Series No. 8 (edited by P. Bhattacharya), INSPEC, London, 1993, p. 61. [117] L. C. Andreani, D. De Nova, S. Di Lernia, M. Geddo, G. Guizzetti, M. Patrini, C. Bocchi, A. Bosacchi, C. Ferrari, and S. Franchi, J. Appl. Phys. 78, 6745 (1995). [118] Z. Hang, D. Yan, F. H. Pollak, G. D. Pettit, and J. M. Woodall, Phys. Rev. B 44, 10546 (1991). [119] C. Alibert, A. Joullie, A. M. Joullie, and C. Ance, Phys. Rev. B 27, 4946 (1983), and references cited therein. [120] A. Bignazzi, E. Grilli, M. Guzzi, C. Bocchi, A. Bosacchi, S. Franchi, and R. Magnanini, Phys. Rev. B 57, 2295 (1998). [121] V. Bellani, M. Geddo, G. Guizzetti, S. Franchi, and R. Magnanini, Phys. Rev. B 59, 12272 (1999). [122] H. Mathieu, D. Auvergne, P. Merle, and K. C. Rustagi, Phys. Rev. B 12, 5846 (1975). [123] R. Ferrini, M. Patrini, and S. Franchi, J. Appl. Phys. 84, 4517 (1998). [124] S. G. Choi, C. J. Palmstrøm, Y. D. Kim, S. L. Cooper, and D. E. Aspnes, J. Appl. Phys. 98, 104108 (2005). [125] N. Kitamura, H. Yamamoto, and T. Wada, Mater. Lett. 15, 89 (1992). [126] S. Isomura, F. G. D. Prat, and J. C. Woolley, Phys. Status Solidi B 65, 213 (1974). [127] X. Yaozhou, Y. Beaulieu, and J. B. Webb, Solid State Commun. 87, 9 (1993). [128] N. Dai, F. Brown, R. E. Doezema, S. J. Chung, K. J. Goldammer, and M. B. Santos, Appl. Phys. Lett. 73, 3132 (1998). [129] S. M. Vishnubhatla, B. Eyglunent, and J. C. Woolley, Can. J. Phys. 47, 1661 (1969). [130] D. Auvergne, J. Camassel, H. Mathieu, and A. Joullie, J. Phys. Chem. Solids 35, 133 (1974). [131] A. P. Roth and E. Fortin, Can. J. Phys. 56, 1468 (1978). [132] R. Rousina, C. Halpin, and J. B. Webb, J. Appl. Phys. 68, 2181 (1990). [133] S. Collins, A. G. Birdwell, R. Glosser, and B. R. Bennett, J. Appl. Phys. 91, 1175 (2002). [134] S. Imai and S. Adachi, Jpn. J. Appl. Phys. 32, 3860 (1993). [135] See, for example, M. Henini, Dilute Nitride Semiconductors, Elsevier, Amsterdam, 2005. [136] U. Tisch, E. Finkman, and J. Salzman, Appl. Phys. Lett. 81, 463 (2002). [137] Y. Zhang, B. Fluegel, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 62, 4493 (2000). [138] Y. Zhang, B. Fluegel, M. C. Hanna, J. F. Geisz, L.-W. Wang, and A. Mascarenhas, Phys. Status Solidi B 240, 396 (2003). [139] W. Shan, W. Walukiewicz, J. W. Ager III, E. E. Haller, J. F. Geisz, D. J. Friedman, J. M. Olson, and S. R. Kurtz, Phys. Rev. Lett. 82, 1221 (1999). [140] W. Shan, W. Walukiewicz, K. M. Yu, J. Wu, J. W. Ager III, E. E. Haller, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 76, 3251 (2000). [141] P. R. C. Kent and A. Zunger, Phys. Rev. Lett. 86, 2613 (2001). [142] P. R. C. Kent and A. Zunger, Phys. Rev. B 64, 115208 (2001). [143] I. A. Buyanova, M. Izadifard, W. M. Chen, H. P. Xin, and C. W. Tu, Phys. Rev. B 69, 201303 (2004). [144] A. Mascarenhas, S. Francoeur, and S. Yoon, in Dilute Nitride Semiconductors (edited by M. Henini), Elsevier, Amsterdam, 2005, p. 179. [145] W. Walukiewicz, W. Shan, J. Wu, K. M. Yu, and J. W. Ager III, in Dilute Nitride Semiconductors (edited by M. Henini), Elsevier, Amsterdam, 2005, p. 325. [146] P. R. C. Kent, in Dilute Nitride Semiconductors (edited by M. Henini), Elsevier, Amsterdam, 2005, p. 393. [147] H. P. Xin, C. W. Tu, Y. Zhang, and A. Mascarenhas, Appl. Phys. Lett. 76, 1267 (2000). [148] I. A. Buyanova, G. Pozina, J. P. Bergman, W. M. Chen, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 81, 52 (2002). [149] G. Y. Rudko, I. A. Buyanova, W. M. Chen, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 81, 3984 (2002). [150] I. A. Buyanova, M. Izadifard, A. Kasic, H. Arwin, W. M. Chen, H. P. Xin, Y. G. Hong, and C. W. Tu, Phys. Rev. B 70, 085209 (2004). [151] D. G. Thomas, J. J. Hopfield, and C. J. Frosch, Phys. Rev. Lett. 15, 857 (1965).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

221

[152] G. Leibiger, V. Gottschalch, M. Schubert, G. Benndorf, and R. Schwabe, Phys. Rev. B 65, 245207 (2002). [153] J. Wu, W. Walukiewicz, K. M. Yu, J. W. Ager III, E. E. Haller, Y. G. Hong, H. P. Xin, and C. W. Tu, Phys. Rev. B 65, 241303 (2002). [154] L. Bellaiche, S.-H. Wei, and A. Zunger, Phys. Rev. B 56, 10233 (1997). [155] M. Weyers, M. Sato, and H. Ando, Jpn. J. Appl. Phys. 31, L853 (1992). [156] G. Pozina, I. Ivanov, B. Monemar, J. V. Thordson, and T. G. Andersson, J. Appl. Phys. 84, 3830 (1998). [157] R. Bhat, C. Caneau, L. Salamanca-Riba, W. Bi, and C. Tu, J. Cryst. Growth 195, 427 (1998). M. Schubert, G. Leibiger, V. Gottschalch, and G. Wagner, J. Appl. Phys. 89, 294 (2001). [158] J. Sik, [159] Y. Zhang, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 63, 161303 (2001). [160] J. Wu, W. Shan, and W. Walukiewicz, Semicond. Sci. Technol. 17, 860 (2002). [161] B. Gil, Solid State Commun. 114, 623 (2000). and M. Schubert, Appl. Phys. Lett. 77, 1650 [162] G. Leibiger, V. Gottschalch, B. Rheinl€ander, J. Sik, (2000). [163] J. Wagner, K. K€ohler, P. Ganser, and N. Herres, Appl. Phys. Lett. 77, 3592 (2000). [164] S. Matsumoto, H. Yaguchi, S. Kashiwase, T. Hashimoto, S. Yoshida, D. Aoki, and K. Onabe, J. Cryst. Growth 221, 481 (2000). and M. Schubert, J. Appl. Phys. 89, 4927 [165] G. Leibiger, V. Gottschalch, B. Rheinl€ander, J. Sik, (2001). [166] U. Tisch, E. Finkman, and J. Salzman, Phys. Rev. B 65, 153204 (2002). [167] A. Pulzara-Mora, E. Cruz-Hernandez, J. Rojas-Ramirez, R. Contreras-Cuerrero, M. MelendezLira, C. Falcony-Guajardo, M. A. Aguilar-Frutis, and M. L opez-L opez, J. Cryst. Growth 301–302, 565 (2007). [168] W. K. Hung, M. Y. Chern, Y. F. Chen, Z. L. Yang, and Y. S. Huang, Phys. Rev. B 62, 13028 (2000). [169] J. D. Perkins, A. Mascarenhas, Y. Zhang, J. F. Geisz, D. J. Friedman, J. M. Olson, and S. R. Kurtz, Phys. Rev. Lett. 82, 3312 (1999). [170] K. Uesugi, I. Suemune, T. Hasegawa, T. Akutagawa, and T. Nakamura, Appl. Phys. Lett. 76, 1285 (2000). [171] R. Chtourou, F. Bousbih, S. B. Bouzid, F. F. Charfi, J. C. Harmand, G. Ungaro, and L. Largeau, Appl. Phys. Lett. 80, 2075 (2002). [172] A. Polimeni, M. Bissiri, A. Augieri, G. B. H. von H€ ogersthal, M. Capizzi, D. Gollub, M. Fischer, M. Reinhardt, and A. Forchel, Phys. Rev. B 65, 235325 (2002). [173] J. Plaza, J. L. Casta~no, B. J. Garcia, H. Carrere, and E. Bedel-Pereira, Appl. Phys. Lett. 86, 121918 (2005). [174] B. S. Ma, F. H. Su, K. Ding, G. H. Li, Y. Zhang, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 71, 045213 (2005). [175] A. Kimura, C. A. Paulson, H. F. Tang, and T. F. Kuech, Appl. Phys. Lett. 84, 1489 (2004). [176] J. Wu, W. Walukiewicz, K. M. Yu, J. D. Denlinger, W. Shan, J. W. Ager III, A. Kimura, H. F. Tang, and T. F. Kuech, Phys. Rev. B 70, 115214 (2004). [177] W. G. Bi and C. W. Tu, Appl. Phys. Lett. 70, 1608 (1997). [178] P. H. Jefferson, T. D. Veal, L. F. J. Piper, B. R. Bennett, C. F. McConville, B. N. Murdin, L. Buckie, G. W. Smith, and T. Ashley, Appl. Phys. Lett. 89, 111921 (2006). [179] W. G. Bi and C. W. Yu, J. Appl. Phys. 80, 1934 (1996). [180] K. M. Yu, W. Walukiewicz, J. Wu, J. W. Beeman, J. W. Ager III, E. E. Haller, W. Shan, H. P. Xin, C. W. Tu, and M. C. Ridgway, J. Appl. Phys. 90, 2227 (2001). [181] H. Naoi, Y. Naoi, and S. Sakai, Solid-State Electron. 41, 319 (1997). [182] D.-K. Shih, H.-H. Lin, L.-W. Sung, T.-Y. Chu,and T.-R. Yang, Jpn. J. Appl. Phys. 42, 375 (2003). [183] M. Kuroda, R. Katayama, S. Nishio, K. Onabe, and Y. Shiraki, Phys. Status Solidi C 0, 2765 (2003). [184] T. D. Veal, L. F. J. Piper, P. H. Jefferson, I. Mahboob, C. F. McConville, M. Merrick, T. J. C. Hosea, B. N. Murdin, and M. Hopkinson, Appl. Phys. Lett. 87, 182114 (2005).

222

PROPERTIES OF SEMICONDUCTOR ALLOYS

[185] J. Wagner, K. K€ohler, P. Ganser, and M. Maier, Appl. Phys. Lett. 87, 051913 (2005). [186] B. N. Murdin, A. R. Adams, P. Murzyn, C. R. Pidgeon, I. V. Bradley, J.-P. R. Wells, Y. H. Matsuda, N. Miura, T. Burke, and A. D. Johnson, Appl. Phys. Lett. 81, 256 (2002). [187] T. D. Veal, I. Mahboob, and C. F. McConville, Phys. Rev. Lett. 92, 13801 (2004). [188] A.-B. Chen and A. Sher, Semiconductor Alloys: Physics and Materials Engineering, Plenum, New York, 1995. [189] F. Saadallah, N. Yacoubi, F. Genty, and C. Alibert, J. Appl. Phys. 94, 5041 (2003). [190] A. G. Thompson, M. Cardona, and K. L. Shaklee, Phys. Rev. 146, 601 (1966). [191] M. G. Craford, R. W. Shaw, A. H. Herzog, and W. O. Groves, J. Appl. Phys. 43, 4075 (1972). [192] A. G. Thompson, J. C. Woolley, and M. Rubenstein, Can. J. Phys. 44, 2927 (1966). [193] K. J. Kim, M. H. Lee, J. H. Bahng, K. Shim, and B. D. Choe, J. Appl. Phys. 84, 3696 (1998). [194] Z. I. Alferov, D. Z. Garbuzov, Y. V. Zhilyaev, and P. S. Kop’ev, Sov. Phys. Semicond. 6, 589 (1992). [195] H. Mathieu, P. Merle, and E. L. Ameziane, Phys. Rev. B 15, 2048 (1977). [196] M. J. Jou, Y. T. Cherng, H. R. Jen, and G. B. Stringfellow, J. Cryst. Growth 93, 62 (1988). [197] S. Loualiche, A. L. Corre, S. Salaun, J. Caulet, B. Lambert, M. Gauneau, D. Lecrosnier, and B. Deveaud, Appl. Phys. Lett. 59, 423 (1991). [198] R. E. Nahory, M. A. Pollack, J. C. DeWinter, and K. M. Williams, J. Appl. Phys. 48, 1607 (1977). [199] M. Yano, Y. Suzuki, T. Ishii, Y. Matsushita, and M. Kimata, Jpn. J. Appl. Phys. 17, 2091 (1978). [200] T. C. McGlinn, T. N. Krabach, and M. V. Klein, Phys. Rev. B 33, 8396 (1986). [201] R. Ferrini, M. Geddo, G. Guizzetti, M. Patrini, S. Franchi, C. Bocchi, F. Germini, A. Baraldi, and R. Magnanini, J. Appl. Phys. 86, 4706 (1999). [202] D. Serries, M. Peter, N. Herres, K. Winkler, and J. Wagner, J. Appl. Phys. 87, 8522 (2000). [203] K. G. Merkel, V. M. Bright, M. A. Marciniak, C. L. A. Cerny, and M. O. Manasreh, Appl. Phys. Lett. 65, 2442 (1994). [204] R. Lukic-Zrnic, B. P. Gorman, R. J. Cottier, T. D. Golding, C. L. Littler, and A. G. Norman, J. Appl. Phys. 92, 6939 (2002). [205] H. Chouaib, C. Bru-Chevallier, G. Guillot, H. Lahreche, and P. Bove, J. Appl. Phys. 98, 123524 (2005). [206] G. A. Antypas and T. O. Yep, J. Appl. Phys. 42, 3201 (1971). [207] R. J. Nicholas, R. A. Stradling, and J. C. Ramage, J. Phys. C: Solid State Phys. 12, 1641 (1979). [208] M. Wada, S. Araki, T. Kudou, T. Umezawa, S. Nakajima, and T. Ueda, Appl. Phys. Lett. 76, 2722 (2000). [209] S. S. Bui, H. P. Lee, and K. M. Yu, Appl. Phys. Lett. 90, 212113 (2007). [210] A. G. Thompson, J. E. Rowe, and M. Rubenstein, Phys. Rev. 40, 3280 (1969). [211] S. G. Choi, C. J. Palmstrøm, Y. D. Kim, D. E. Aspnes, H. J. Kim, and Y.-C. Chang, Appl. Phys. Lett. 91, 041917 (2007). [212] E. H. Reihlen, M. J. Jou, Z. M. Fang, and G. B. Stringfellow, J. Appl. Phys. 68, 4604 (1990). [213] W. J. Duncan, A. S. M. Ali, E. M. Marsh, and P. C. Spurdens, J. Cryst. Growth 143, 155 (1994). [214] J. C. Woolley and J. Warner, Can. J. Phys. 42, 1879 (1964). [215] G. B. Stringfellow and P. E. Greene, J. Electrochem. Soc. 118, 805 (1971). [216] W. Dobbelaere, J. D. Boeck, and G. Borghs, Appl. Phys. Lett. 55, 1856 (1989). [217] H. Y. Deng and N. Dai, Phys. Rev. B 73, 113102 (2006). [218] S. Elies, A. Krier, I. R. Cleverley, and K. Singer, J. Phys. D: Appl. Phys. 26, 159 (1993). [219] M. A. Marciniak, R. L. Hengehold, Y. K. Yeo, and G. W. Turner, J. Appl. Phys. 84, 480 (1998). [220] B. Bansal, V. K. Dixit, V. Venkataraman, and H. L. Bhat, Appl. Phys. Lett. 82, 4720 (2003). [221] V. K. Dixit, B. Bansal, V. Venkataraman, H. L. Bhat, K. S. Chandrasekharan, and B. M. Arora, J. Appl. Phys. 96, 4989 (2004). [222] Y. Z. Gao, X. Y. Gong, Y. H. Chen, and T. Yamaguchi, Proc. SPIE 6029, 60291I (2006). [223] Y. G. Hong, A. Nishikawa, and C. W. Tu, Appl. Phys. Lett. 83, 5446 (2003). [224] I. A. Buyanova, M. Izadifard, W. M. Chen, Y. G. Hong, and C. W. Tu, Appl. Phys. Lett. 88, 031907 (2006).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

223

[225] K. I. Lin, T. S. Wang, Y. T. Lu, and J. S. Hwang, J. Appl. Phys. 99, 056103 (2006). [226] K. I. Lin and J. S. Hwang, Appl. Phys. Lett. 89, 192116 (2006). [227] A. E. Zhukov. A. R. Kovsh, E. S. Semenova, V. M. Ustinov, L. Wei J.-S. Wang, and J. Y. Chi, Semicond. 36, 899 (2002). [228] Z. Pan, L. H. Li, Y. W. Lin, B. Q. Sun, D. S. Jiang, and W. K. Ge, Appl. Phys. Lett. 78, 2217 (2001). [229] S. A. Choulis, T. J. C. Hosea, S. Tomic, M. Kamal-Saadi, A. R. Adams, E. P. O’Reilly, B. A. Weinstein, and P. J. Klar, Phys. Rev. B 66, 165321 (2002). [230] A. Polimeni, M. Capizzi, M. Geddo, M. Fischer, M. Reinhardt, and A. Forchel, Phys. Rev. B 63, 195320 (2001). [231] H. D. Sun, M. D. Dawson, M. Othman, J. C. L. Yong, J. M. Rorison, P. Gilet, L. Grenouillet, and A. Million, Appl. Phys. Lett. 82, 376 (2003). [232] D. Serries, T. Geppert, P. Ganser, M. Maier, K. K€ohler, N. Herres, and J. Wagner, Appl. Phys. Lett. 80, 2448 (2002). [233] C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002), and references cited therein. [234] P. Perlin, S. G. Subramanya, and D. E. Mars, Appl. Phys. Lett. 73, 3703 (1998). [235] C. Skierbiszewski, P. Erlin, P. Wisniewski, T. Suski, J. F. Geisz, K. Hingerl, W. Jantsch, D. E. Mars, and W. Walukiewicz, Phys. Rev. B 65, 035207 (2001). [236] M. M. E. Fahmi, A. Khan, J. A. Griffin, G. L. Harris, L. H. Robins, A. G. Birdwell, Y.-S. Kang, D. J. Smith, T. Steiner, and S. N. Mohammad, J. Appl. Phys. 94, 7576 (2003). [237] Y.-S. Kang, L. H. Robins, A. G. Birdwell, A. J. Shapiro, W. R. Thurber, M. D. Vaudin, M. M. E. Fahmi, D. Bryson, and S. N. Mohammad, J. Appl. Phys. 98, 093714 (2005). [238] L. Bellaiche, Appl. Phys. Lett. 75, 2578 (1999). [239] K. M. Yu, W. Walukiewicz, J. W. Ager III, D. Bour, R. Farshchi, O. D. Dubon, S. X. Li, I. D. Sharp, and E. E. Haller, Appl. Phys. Lett. 88, 092110 (200). [240] J. H. Herrera-Perez, M. B. Z. Morosini, and N. P. Patel, in Proceedings of the 5th Brazilian School on Semiconductor Physics (edited by J. R. Leite, A. Fazzio, and A. S. Chaves), World Scientific, Singapore, 1991, p. 395. [241] N. Yacoubi, A. Hafaiedh, and A. Joullie, Appl. Opt. 33, 7171 (1994). [242] D. O. T. Filho, I. F. L. Dias, E. Laureto, J. L. Duarte, S. A. Louren˛c o, L. C. Po˛c as, S. S. Prabhu, and J. Klem, J. Appl. Phys. 97, 123702 (2005). [243] S. P. Svensson, D. M. Gill, and P. N. Uppal, J. Appl. Phys. 81, 1422 (1997). [244] N. A. Charykov, A. M. Litvak, K. D. Moiseev, and Y. P. Yakovlev, Proc. SPIE 1512, 198 (1991). [245] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992. [246] S. Shirakata, M. Kondo, T. Nishino, and Y. Hamakawa, Jpn. J. Appl. Phys. 25, 435 (1986). [247] G. P. Donati, R. Kaspi, and K. J. Malloy, J. Appl. Phys. 94, 5814 (2003). [248] L. I. Kamlet and F. L. Terry, Jr., J. Electron. Mater. 24, 2005 (1995). [249] C. Reh and G. Weiser, Phys. Rev. B 65, 035321 (2001). [250] J. C. DeWinter, M. A. Pollack, A. K. Srivastava, and J. L. Zyskind, J. Electron. Mater. 14, 729 (1985). [251] T. I. Voronina, T. S. Lagunova, M. P. Mikhailova, M. A. Sipovskaya, V. V. Sherstnev, and Y. P. Yakoviev, Sov. Phys. Semicond. 25, 167 (1991). [252] M. P. Mikhailova and A. N. Titkov, Semicond. Sci. Technol. 9, 1279 (1994). [253] M. J. Cherng, G. B. Stringfellow, D. W. Kisker, A. K. Srivastava, and J. L. Zyskind, Appl. Phys. Lett. 48, 419 (1986). [254] T. Mei, J. Appl. Phys. 101, 013520 (2007). [255] S. Iyer, S. Hegde, K. K. Bajaj, A. Abul-Fadl, and W. Mitchel, J. Appl. Phys. 73, 3958 (1993). [256] M. Mu~noz, F. H. Pollak, M. B. Zakia, N. B. Patel, and J. L. Herrera-Perez, Phys. Rev. B 62, 16600 (2000). [257] X. Gong, H. Kan, T. Yamaguchi, I. Suzuki, M. Aoyama, M. Kumagawa, N. L. Rowell, A. Wang, and R. Rinfret, Jpn. J. Appl. Phys. 33, 1740 (1994).

224

PROPERTIES OF SEMICONDUCTOR ALLOYS

[258] D. J. Mowbray, O. P. Kowalski, M. Hopkinson, and J. P. R. David, Appl. Phys. Lett. 65, 213 (1994). [259] S. P. Najda, A. H. Kean, M. D. Dawson, and G. Duggan, J. Appl. Phys. 77, 3412 (1995). [260] M. Schubert, J. A. Woollam, G. Leibiger, B. Rheinl€ander, I. Pietzonka, T. Sab, and V. Gottschalch, J. Appl. Phys. 86, 2025 (1999). [261] K. Asami, H. Asahi, S. Gonda, Y. Kawamura, and H. Tanaka, Solid State Commun. 70, 33 (1989). [262] D. S. Cao, A. W. Kimball, and G. B. Stringfellow, J. Appl. Phys. 67, 739 (1990). [263] S. Adachi, S. Ozaki, M. Sato, and K. Ohtsuka, Jpn. J. Appl. Phys. 35, 537 (1996). [264] S. Ozaki, S. Adachi, M. Sato, and K. Ohtsuka, J. Appl. Phys. 79, 439 (1996). [265] H. Lee, M. V. Klein, D. E. Aspnes, C. P. Kuo, M. Peanasky, and M. G. Craford, J. Appl. Phys. 73, 400 (1993). [266] A. D. Prins, J. L. Sly, A. T. Meney, D. J. Dunstan, E. P. O’Reilly, A. R. Adams, and A. Valster, J. Phys. Chem. Solids 56, 349 (1995). [267] J. Harada, T. Kobayashi, A. D. Prins, and D. J. Dunstan, Phys. Status Solidi B 235, 505 (2003). [268] J. I. Davies, A. C. Marshall, M. D. Scott, and R. J. M. Griffiths, Appl. Phys. Lett. 53, 276 (1988). [269] C. Cacciatore, D. Campi, C. Coriasso, C. Rigo, and C. Alibert, Thin Solid Films 197, 1 (1991). [270] W. F. Tseng, J. Comas, B. Steiner, G. Metze, A. Cornfeld, P. B. Klein, D. K. Gaskill, W. Xia, and S. S. Lau, Mater. Res. Soc. Symp. Proc. 240, 117 (1992). [271] R. F. Kopf, H. P. Wei, A. P. Perley, and G. Livescu, Appl. Phys. Lett. 60, 2386 (1992). [272] P. Parayanthal, C. S. Ro, F. H. Pollak, C. R. Stanley, G. W. Wicks, and L. F. Eastman, Appl. Phys. Lett. 43, 109 (1983). [273] J.-W. Pan, J.-L. Shieh, J.-H. Gau, J.-I. Chyi, J.-C. Lee, and K.-J. Ling, J. Appl. Phys. 78, 442 (1995). [274] S. N. Grinyaev, L. M. Dolginov, M. A. Il’in, Y. N. Korchagin, A. I. Lukomskiı, and V. A. Chaldyshev, Sov. Phys. Semicond. 16, 467 (1982). [275] H. Mani, E. Tournie, J. L. Lazzari, C. Alibert, A. Joullie, and B. Lambert, J. Cryst. Growth 121, 463 (1992). [276] L.-C. Chen, W.-J. Ho, and M.-C. Wu, Jpn. J. Appl. Phys. 38, 1314 (1999). [277] Y. R. Ryu, T. S. Lee, J. A. Lubguban, A. B. Corman, H. W. White, J. H. Leem, M. S. Han, Y. S. Park, C. J. Youn, and W. J. Kim, Appl. Phys. Lett. 88, 052103 (2006). [278] M. S. Han, J. H. Kim, T. S. Jeong, J. M. Park, C. J. Youn, J. H. Leem, and Y. R. Ryu, J. Cryst. Growth 303, 506 (2007). [279] T. Makino, Y. Segawa, M. Kawasaki, A. Ohtomo, R. Shiroki, K. Tamura, T. Yasuda, and H. Koinuma, Appl. Phys. Lett. 78, 1237 (2001). [280] R. Schmidt-Grund, M. Schubert, B. Rheinl€ander, D. Fritsch, H. Schmidt, E. M. Kaidashev, M. Lorenz, C. M. Herzinger, and M. Grundmann, Thin Solid Films 455–456, 500 (2004). [281] K. Koike, K. Hama, I. Nakashima, G. Takada, K. Ogata, S. Sasa, M. Inoue, and M. Yano, J. Cryst. Growth 278, 288 (2005). [282] R. Schmidt-grund, A. Carstens, B. Rheinl€ander, D. Spemenn, H. Hochmut, G. Zimmermann, M. Lorenz, and M. Grundmann, J. Appl. Phys. 99, 123701 (2006). [283] N. B. Chen and C. H. Sui, Mater. Sci. Eng. B 126, 16 (2006). [284] J. A. Sans and A. Segura, High Pressure Res. 24, 119 (2004). [285] J. Ishihara, A. Nakamura, S. Shigemori, T. Aoki, and J. Temmyo, Appl. Surf. Sci. 244, 381 (2005), and references cited therein. [286] X. J. Wang, I. A. Buyanova, W. M. Chen, M. Izadifard, S. Rawal, D. P. Norton, S. J. Pearton, A. Osinsky, J. W. Dong, and A. Dabiran, Appl. Phys. Lett. 89, 151909 (2006). [287] H. S. Kang, J. W. Kim, J. H. Kim, S. Y. Lee, Y. Li, J.-S. Lee, J. K. Lee, M. A. Nastasi, S. A. Crooker, and Q. X. Jia, J. Appl. Phys. 99, 066113 (2006). [288] H. C. Ong and J. Y. Dai, Appl. Phys. Lett. 81, 1444 (2002). [289] K. Ichino, K. Ueyama, M. Yamamoto, H. Kariya, H. Miyata, H. Misasa, M. Kitagawa, and H. Kobayashi, J. Appl. Phys. 87, 4249 (2000). [290] G. K. Padam, G. L. Malhotra, and S. U. M. Rao, J. Appl. Phys. 63, 770 (1988). [291] A. Beliveau and C. Carlone, Phys. Rev. B 41, 9860 (1990).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS [292] [293] [294] [295] [296] [297] [298] [299] [300] [301] [302] [303] [304] [305] [306] [307] [308] [309] [310] [311] [312] [313] [314] [315] [316] [317] [318] [319] [320] [321] [322] [323] [324]

225

V. Kumar, V. Singh, S. K. Sharma, and T. P. Sharma, Opt. Mater. 11, 29 (1998). A. M. Salem, Appl. Phys. A 74, 205 (2002). T. Yokogawa, T. Ishikawa, J. L. Merz, and T. Taguchi, J. Appl. Phys. 75, 2189 (1994). M. R. Muhamad, Jpn. J. Appl. Phys. 32, 3385 (1993). A. Kremheller, A. K. Levine, and G. Gashurov, J. Electrochem. Soc. 107, 12 (1960). E. S. Rittner and J. H. Schulman, J. Phys. Chem. 47, 537 (1943). K. Wilmers, T. Wethkamp, N. Esser, C. Cobet, W. Richter, V. Wagner, H. Lugauer, F. Fischer, T. Gerhard, M. Keim, and M. Cardona, J. Electron. Mater. 28, 670 (1999). A. Bukaluk, A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Ł e˛ gowski, H. M e˛ czynska, and J. Szatkowski, Appl. Surf. Sci. 175–176, 531 (2001). G. P. Srivastava, H. M. T€ut€unc€u, and N. G€unhan, Phys. Rev. B 70, 085206 (2004). C. Chauvet, E. Tournie, and J.-P. Faurie, Phys. Rev. B 61, 5332 (2000). C. Chauvet, E. Tournie, and J.-P. Faurie, J. Cryst. Growth 214/215, 95 (2000). H. Lee, I.-Y. Kim, J. Powell, D. E. Aspnes, S. Lee, F. Peiris, and J. K. Furdyna, J. Appl. Phys. 88, 878 (2000). S. V. Ivanov, O. V. Nekrutkina, S. V. Sorokin, V. A. Kaygorodov, T. V. Shubina, A. A. Toropov, P. S. Kop’ev, G. Reuscher, V. Wagner, J. Geurts, A. Waag, and G. Landwehr, Appl. Phys. Lett. 78, 404 (2001). O. Maksimov, M. Mu~noz, and M. C. Tamargo, Microelectron. J. 37, 19 (2006). P. J. Huang, P. Sitarek, Y. S. Huang, O. Maksimov, M. C. Tamargo, F. Firszt, and H. M e˛ czy nska, Phys. Status Solidi C 3, 738 (2006). A. A. Wronkowska, A. Wronkowski, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, A. Marasek, and W. Paszkowicz, Phys. Status Solidi C 1, 641 (2004). F. Firszt, S. Ł e˛ gowski, H. M e˛ czynska, H. L. Oczkowski, W. Osi nska, J. Szatkowski, W. Paszkowicz, and Z. M. Spolnik, J. Cryst. Growth 159, 167 (1996). B. Jobst, D. Hommel, U. Lunz, T. Gerhard, and G. Landwehr, Appl. Phys. Lett. 69, 97 (1996). H. Okuyama, Y.Kishita, and A. Ishibashi, Phys. Rev. B 57, 2257 (1998). K. J. Kim, M. H. Lee, J. H. Bahng, C. Y. Kwak, and E. Oh, Solid State Commun. 105, 17 (1998). M. Sohel, M. Mu~noz, and M. C. Tamargo, Appl. Phys. Lett. 85, 2794 (2004). R. P€assler, F. Blaschta, E. Griebl, K. Papagelis, B. Haserer, T. Reisinger, S. Ves, and W. Gebhardt, Phys. Status Solidi B 204, 685 (1997). A. Gapinski and W. Bała, Proc. SPIE 3725, 72 (1999). W.-T. Kim, Phys. Rev. B 59, 4572 (1999). A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, and J. Szatkowski, Vacuum 63, 233 (2001). F. Firszt, A. A. Wronkowska, A. Wronkowski, S. Ł e˛ gowski, A. Marasek, H. M e˛ czy nska, M. Pawlak, W. Paszkowicz, K. Strzałkowski, and A. J. Zakrzewski, Cryst. Res. Technol. 40, 386 (2005). D.-T. Kim, S.-A. Park, W.-J. Jeong, C.-C. Park, M.-S. Jin, and C.-D. Kim, Phys. Status Solidi C 3, 2665 (2006). V. A. Kaygorodov, I. V. Sedova, S. V. Sorokin, A. A. Sitnikova, O. V. Nekrutkina, T. V. Shubina, A. A. Toropov, V. S. Sorokin, and S. V. Ivanov, Phys. Status Solidi B 229, 19 (2002). C.-D. Kim, D.-H. Shin, H.-H. Jang, H.-M. Jeong, D.-T. Kim, C.-S. Yoon, H.-L. Park, and W.-T. Kim, J. Appl. Phys. 85, 7972 (1999). P. J. Huang. Y. S. Huang, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, and K. K. Tiong, J. Phys.: Condens. Matter 19, 266002 (2007). A. S. Nasibov, Y. V. Korostelin, P. V. Shapkin, L. G. Suslina, D. L. Fedorov, and L. S. Markov, Solid State Commun. 71, 867 (1989). N. Samarth, H. Luo, J. K. Furdyna, R. G. Alonso, Y. R. Lee, A. K. Ramdas, S. B. Qadri, and N. Otsuka, Appl. Phys. Lett. 56, 1163 (1990). Y. D. Kim, M. V. Klein, S. F. Ren, Y. C. Chang, H. Luo, N. Samarth, and J. K. Furdyna, Phys. Rev. B 49, 7262 (1994).

226

PROPERTIES OF SEMICONDUCTOR ALLOYS

[325] U. Lunz, J. Kuhn, F. Goschenhofer, U. Sch€ussler, S. Einfeldt, C. R. Becker, and G. Landwehr, J. Appl. Phys. 80, 6861 (1996). [326] J. Lee, F. Flack, N. Samarth, and R. W. Collins, Appl. Opt. 36, 5372 (1997). [327] L. Malikova, W. Krystek, F. H. Pollak, N. Dai, A. Cavus, and M. C. Tamargo, Phys. Rev. B 54, 1819 (1996). [328] M.-C. Kuo, K.-C. Chiu, T.-H. Shin, Y.-J. Lai, C.-S. Yang, W.-K. Chen, D.-S. Chuu, M.-C. Lee, W.-C. Chou, S.-Y. Jeng, Y.-T. Shin, and W.-H. Lan, Jpn. J. Appl. Phys. 43, 5145 (2004). [329] A. Kalb and V. Leute, Phys. Status Solidi A 5, K199 (1971). [330] C. J. Summers and J. G. Broerman, Phys. Rev. B 21, 559 (1980). [331] N. Himei and J. Muto, J. Mater. Sci.: Mater. Electron. 11, 145 (2000). [332] V. B. Pujari, S. H. Mane, V. S. Karande, J. S. Dargad, and L. P. Deshmukh, Mater. Chem. Phys. 83, 10 (2004). [333] I. N. Borisov, P. S. Kireev, V. V. Mikhailin, and V. M. Bezborodova, Sov. Phys. Semicond. 5, 734 (1971). [334] K. Kumazaki, L. Vi~na, C. Umbach, and M. Cardona, Phys. Status Solidi B 156, 371 (1989). [335] O. Maksimov and M. C. Tamargo, Appl. Phys. Lett. 79, 782 (2001). [336] M. R. Buckley, F. C. Peiris, O. Maksimov, M. Mu~ noz, and M. C. Tamargo, Appl. Phys. Lett. 81, 5156 (2002). [337] M. Mu~noz, O. Maksimov, M. C. Tamargo, M. R. Buckley, and F. C. Peiris, Phys. Status Solidi C 1, 706 (2004). [338] J. Zakrzewski, Proc. SPIE 5953, 595307 (2005). [339] S. G. Parker, A. R. Reinberg, J. E. Pinnell, and W. C. Holton, J. Electrochem. Soc. 118, 979 (1971). [340] D. Barbier, B. Montegu, and A. Laugier, Solid State Commun. 28, 525 (1978). [341] S.-J. Chung, Y. Kwon, C.-S. Yoon, B.-H. Kim, D. Cha, C.-D. Kim, W.-T. Kim, and C. U. Hong, J. Phys. Chem. Solids 60, 799 (1999). [342] A. J. Franz, F. C. Peiris, X. Liu, U. Bindley, and J. K. Furdyna, Phys. Status Solidi B 241, 507 (2004). [343] K. Itoh, J. Phys. Soc. Jpn 22, 1119 (1967). [344] M. Luttmann, F. Bertin, and A. Chabli, J. Appl. Phys. 78, 3387 (1995). [345] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, I. Miotkowski, and A. K. Ramdas, Appl. Phys. Lett. 71, 249 (1997). [346] Y. S. Ihn, T. J. Kim, T. H. Ghong, Y. D. Kim, D. E. Aspnes, and J. Kossut, Thin Solid Films 455–456, 222 (2004). [347] B. Freytag, J. Phys.: Condens. Matter 6, 9875 (1994). [348] K. Saito, A. Ebina, and T. Takahashi, Solid State Commun. 11, 841 (1972). [349] V. A. Tyagai, O. V. Snitko, V. N. Bondarenko, N. I. Vitrikhovskii, V. B. Popov, and A. N. Krasiko, Sov. Phys. Solid State 16, 885 (1974). [350] V. V. Sobolev, O. G. Maksimova, and S. G. Kroitoru, Phys. Status Solidi B 499 (1981). [351] S. Adachi and T. Kimura, Jpn. J. Appl. Phys. 32, 3496 (1993). [352] O. Castaing, R. Granger, J. T. Benhlal, and R. Triboulet, J. Phys.: Condens. Matter 8, 5757 (1996). [353] K. P. Rao, O. M. Hussain, K. T. R. Reddy, P. S. Reddy, S. Uthanna, B. S. Naidu, and P. J. Reddy, Opt. Mater. 5, 63 (1996). [354] P. D. Paulson, B. E. McCandless, and R. W. Birkmire, J. Appl. Phys. 95, 3010 (2004). [355] A. Kisiel, Acta Phys. Polon. A 38, 691 (1970). [356] E. M. Larramendi, E. Puron, and O. de Melo, Semicond. Sci. Technol. 17, 8 (2002). [357] F. G. Sanchez-Almazan, H. Navarro-Contreras, G. Ramırez-Flores, M. A. Vidal, O. Zelaya-Angel, M. E. Rodrıguez, and R. Baquero, J. Appl. Phys. 79, 7713 (1996). [358] O. Zelaya-Angel, J. G. Mendoza-Alvarez, M. Becerril, H. Navarro-Contreras, and L. TiradoMejia, J. Appl. Phys. 95, 6284 (2004). [359] Y. T. Shih, W. C. Fan, C. S. Yang, M. C. Kuo, and W. C. Chou, J. Appl. Phys. 94, 3791 (203). [360] B. Toulouse, R. Granger, S. Rolland, and R. Triboulet, J. Phys. 48, 247 (1987).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

227

[361] D. Lemoine, K. H. Khelladi, O. Castaing, J. Benhlal, A. Quemerais, I. Pollini, R. Triboulet, and R. Granger, Mater. Sci. Eng. B 28, 39 (1994). [362] F. El-Akkad and A. R. Farhan, J. Phys. D: Appl. Phys. 28, 1958 (1995). [363] O. Casting, J. T. Benhlal, R. Granger, and R. Triboulet, J. Phys. I France 6, 907 (1996). [364] V. G. Sredin, V. G. Savitskiı, Y. V. Danilyuk, M. V. Miliyanchuk, and I. V. Petrovich, Sov. Phys. Semicond. 15, 249 (1981). [365] J. P. Laurenti, J. Camassel, A. Bouhemadou, B. Toulouse, R. Legros, and A. Lusson, J. Appl. Phys. 67, 6454 (1990). [366] J. Chu, Z. Mi, and D. Tang, Infrared Phys. 32, 195 (1991). [367] A. Rodzik and A. Kisiel, J. Phys. C: Solid State Phys. 16, 203 (1983). [368] A. Moritani, K. Taniguchi, C. Hamaguchi, J. Nakai, R. Ueda, and O. Ohtsuki, J. Phys. Soc. Jpn. 31, 945 (1971). [369] L. Vi~na, C. Umbach, M. Cardona, and L. Vodopyanov, Phys. Rev. B 29, 6752 (1984). [370] H. Arwin and D. E. Aspnes, J. Vac. Sci. Technol. A 2, 1316 (1984). [371] M. W. Scott, J. Appl. Phys. 40, 4077 (1969). [372] G. L. Hansen, J. L. Schmit, and T. N. Casselman, J. Appl. Phys. 53, 7099 (1982). [373] A. Ksendzov, F. H. Pollak, J. A. Wilson, and V. A. Cotton, J. Appl. Phys. 66, 5528 (1989). [374] C. C. Kim and S. Sivananthan, J. Electron. Mater. 26, 561 (1997). [375] C.-Y. Moon, S.-H. Wei, Y. Z. Zhu, and G. D. Chen, Phys. Rev. B 74, 233202 (2006). [376] B. K. Meyer, A. Polity, B. Farangis, Y. He, D. Hasselkamp, T. Kr€amer, and C. Wang, Appl. Phys. Lett. 85, 4929 (2004). [377] Y. Nabetani, T. Mukawa, Y. Ito, T. Kato, and T. Matsumoto, Appl. Phys. Lett. 83, 1148 (2003). [378] W. Shan, W. Walukiewicz, J. W. Ager III, K. M. Yu, J. Wu, E. E. Haller, Y. Nabetani, T. Murakawa, Y. Ito, and T. Matsumoto, Appl. Phys. Lett. 83, 299 (2003). [379] A. Polimeni, M. Capizzi, Y. Nabetani, Y. Ito, K. Kato, T. Matsumoto, and T. Hirai, Appl. Phys. Lett. 84, 3304 (2004). [380] A. Ebina, E. Fukunaga, and T. Takahashi, Phys. Rev. B 10, 2495 (1974). [381] H. Araki, H. Kanie, and M. Sano, Jpn. J. Appl. Phys. 33, 235 (1994). [382] E. Griebl, G. F. Sch€otz, C. Birzer, W. Kerner, T. Reisinger, B. Hahn, and W. Gebhardt, Acta Phys. Polon. A 88, 995 (1995). [383] P. R. Newbury, K. Shahzad, J. Petruzzello, and D. A. Cammack, J. Appl. Phys. 66, 4950 (1989). [384] R. Hill and D. Richardson, J. Phys. C: Solid State Phys. 6, L115 (1973). [385] Y.-M. Yu, S. Nam, J.-K. Rhee, B. O, K.-S. Lee, and Y. D. Choi, J. Cryst. Growth 210, 521 (2000). [386] W. Walukiewicz, W. Shan, K. M. Yu, J.W. Ager III, E. E. Haller, I. Miotkowski, M. J. Seong, H. Alawadhi, and A. K. Ramdas, Phys. Rev. Lett. 85, 1552 (2000). [387] C. Y. Bang, M. S. Lee, T. J. Kim, Y. D. Kim, D. E. Aspnes, Y. M. Yu, B. O, and Y. D. Choi, J. Kor. Phys. Soc. 39, 462 (2001). [388] S. Larach, R. E. Shrader, and C. F. Stocker, Phys. Rev. 108, 587 (1957). [389] A. Ebina, M. Yamamoto, and T. Takahashi, Phys. Rev. B 6, 3786 (1972). [390] M. J. S. P. Brasil, R. E. Nahory, F. S. Turco-Sandroff, H. L. Gilchrist, and R. J. Martin, Appl. Phys. Lett. 58, 2509 (1991). [391] C.-H. Su, S. Feth, S. Zhu, S. L. Lehoczky, and L. J. Wang, J. Appl. Phys. 88, 5148 (2000). [392] H. Lee, S. M. Kim, B. Y. Seo, E. Z. Seong, S. H. Choi, S. Lee, and J. K. Furdyna, Appl. Phys. Lett. 77, 2997 (2000). [393] A. Naumov, H. Stanzl, K. Wolf, S. Lankes, and W. Gebhardt, J. Appl. Phys. 74, 6178 (1993). [394] J. Wu, W. Walukiewicz, K. M. Yu, W. Shan, J. W. Ager III, E. E. Haller, I. Miotkowski, A. K. Ramdas, and C.-H. Su, Phys. Rev. B 68, 033206 (2003). [395] V. N. Bondarenko, N. I. Vitrikhovskii, and V. A. Tyagai, Sov. Phys. Solid State 13, 1854 (1972). [396] G. Perna, S. Pagliara, V. Capozzi, M. Ambrico, and M. Pallara, Solid State Commun. 114, 161 (2000). [397] R. L. Hengehold and C. R. Fraime, Phys. Rev. 174, 808 (1968).

228 [398] [399] [400] [401] [402] [403] [404] [405] [406] [407] [408] [409] [410] [411] [412] [413] [414] [415] [416] [417]

PROPERTIES OF SEMICONDUCTOR ALLOYS D. W. Lane, Sol. Ener. Mater. Sol. Cells 90, 1169 (2006). K. Ohata, J. Saraie, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1641 (1973). K. Wei, F. H. Pollak, J. L. Freeouf, D. Shvydka, and A. D. Compaan, J. Appl. Phys. 85, 7418 (1999). P. J. Sebastian and V. Sivaramakrishnan, J. Cryst. Growth 112, 421 (1991). M. Schenk and C. Silber, J. Mater. Sci.: Mater. Electron. 9, 295 (1998). Z. C. Feng, P. Becla, L. S. Kim, S. Perkowitz, Y. P. Feng, H. C. Poon, K. P. Williams, and G. D. Pitt, J. Cryst. Growth 138, 239 (1994). G. Brill, Y. Chen, P. M. Amirtharaj, W. Sarney, D. Chandler-Horowitz, and N. K. Dhar, J. Electron. Mater. 34, 655 (2005). J. M. Gaines, R. R. Drenten, K. W. Haberern, T. Marshall, P. Mensz, and J. Petruzzello, Appl. Phys. Lett. 62, 2462 (1993). U. Lunz, B. Jobst, S. Einfeldt, C. R. Becker, D. Hommel, and G. Landwehr, J. Appl. Phys. 77, 5377 (1995). H. J. Chen, D. Y. Lin, Y. S. Huang, R. C. Tu, Y. K. Su, and K. K. Tiong, Semicond. Sci. Technol. 14, 85 (1999). K. Naniwae, H. Iwata, and K. Yashiki, Appl. Phys. Lett. 74, 3984 (1999). K. Shim, H. Rabitz, J.-H. Chang, and T. Yao, J. Cryst. Growth 214/215, 350 (2000). V. Wagner, A. Fleszar, J. Geurts, G. Reusher, M. Keim, A. Waag, G. Landwehr, K. Wilmers, N. Esser, and W. Richter, J. Cryst. Growth 214/215, 340 (2000). K. Godo, H. Makino, M. W. Cho, J. H. Chang, Y. Yamazaki, T. Yao, M. Y. Shen, and T. Goto, Appl. Phys. Lett. 79, 4168 (2001). P. J. Huang, H. P. Hsu, Y. S. Huang, F. Firzt, S. L e˛ gowski, H. M e˛ czy nska, A. Marasek, and K. K. Tiong, J. Appl. Phys. 102, 083515 (2007). Y. T. Liu, P. Sitarek, Y. S. Huang, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, A. Marasek, W. Paszkowicz, and K. K. Tiong, J. Appl. Phys. 98, 083519 (2005). A. A. Wronkowska, F. Firszt, H. Arwin, A. Wronkowski, M. Wakula, K. Strzalkowski, and W. Paszkowicz, Phys. Status Solidi C 3, 1193 (2006). J. W. Wang, P. J. Huang, H. P. Hsu, Y. S. Huang, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, A. Marasek, and K. K. Tiong, J. Appl. Phys. 101, 103539 (2007). C.-H. Hsieh, Y.-S. Huang, C.-H. Ho, K.-K. Tiong, M. Mu~ noz, O. Maksimov, and M. C. Tamargo, Jpn. J. Appl. Phys. 43, 459 (2004). O. Maksimov, M. Mu~noz, W. H. Wang, M. C. Tamargo, and N. Samarth, Phys. Status Solidi B 241, R5 (2004).

7 Energy-band Structure: Effective Masses 7.1 INTRODUCTORY REMARKS 7.1.1 Electron Effective Mass The constant-energy surface in semiconductors can be defined by E¼

h2 k2y h2 k2z 2 k2x h þ þ 2mx 2my 2mz

ð7:1Þ

where the electron at the center of the BZ has a spherical constant-energy surface (i.e. mx ¼ my ¼ mz), while there are six constant-energy ellipsoids along the principal diagonal [100] and its equivalent directions and eight ellipsoids along the h111i directions [1]. In such ellipsoidal constant-energy surfaces, Equation (7.1) can be simply written as E¼

2 k2t h h2 k2l þ mt 2ml

ð7:2Þ

The two masses ml and mt in Equation (7.2) are the longitudinal mass and transverse mass, respectively, because ml (mz) is defined along the h100i axis (X valley) and along the h111i axis (L valley), whereas mt (mx ¼ my) is defined in a plane transverse to the said axis. The longitudinal effective mass, ml, is usually much larger than its counterparts mt. The DOS effective mass mae for electrons in the CB minima a ¼ G, X or L is given by 2=3

1=3

mae ¼ N 2=3 mta mla

ð7:3Þ

where N is the number of equivalent a minima (N ¼ 1 for the G minimum, N ¼ 3 for the X minima and N ¼ 4 for the L minima). The DOS mass can be used for DOS calculations. The conductivity effective mass mac , which can be used for conductivity or mobility calculations, is written as mac ¼

3mta mla mta þ 2mla

ð7:4Þ

Since mtG ¼ mlG, we have the relationship mGe ¼ mGc at the a ¼ G minimum. In hexagonal semiconductors, the CB electron has an ellipsoidal constant-energy surface, not a spherical surface, even at the zone center (G)

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

230

PROPERTIES OF SEMICONDUCTOR ALLOYS

jj m? e mx ¼ my 6¼ mz me

ð7:5Þ

Thus, mGe 6¼ mGc holds in such anisotropic semiconductors, but its difference is very small. We summarize in Table 7.1 the G-valley electron effective mass mGe for a number of cubic group-IV, III–V and II–VI semiconductors. Table 7.2 also summarizes the G-valley electron effective masses for some wurtzite III–V and II–VI semiconductors. The mGe values for InN, BeSe and BeTe in Table 7.1 and those for InN, BeO, BeSe and CdTe in Table 7.2 are obtained using the mGe versus E0 relationships described in Section 7.1.2 of Adachi [1]. The InN values in Table 7.2 are taken from Hofmann et al. [2]. The electron effective masses in the X (D) and L minima for some cubic group-IVand III–V semiconductors are listed in Table 7.3. The corresponding DOS and conductivity masses are listed in Table 7.4.

7.1.2 Hole Effective Mass The effective Hamiltonian is generally derived from a kp theory or from the theory of invariants developed by Bir and Pikus. The effective Hamiltonians for the CB and VB in the Table 7.1 Electron effective mass mGe for some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

BN (zb) BP (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

mGe /m0 0.36–2.030a 0.188a 0.038 0.058b 0.449a

System

Material

II–VI

BeSe (zb) BeTe (zb) MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

0.752a 0.150a 0.0499a 0.26a 0.220a 0.124 0.14 0.15 0.114 0.067 0.039 0.03a 0.07927 0.024 0.013

Calculated or estimated The sign is chosen positive for a normal band structure like that of Ge c The sign is chosen positive for a normal band structure like that of CdTe a b

mGe /m0 0.28a 0.21a 0.35a 0.225a 0.20a 0.17a 0.20 0.137 0.117 0.21 0.14a 0.112 0.090 0.006a,c 0.042a,c 0.028c

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

231

k

G Table 7.2 G-valley electron effective masses, m? e , me and me , for some wurtzite III–V and II–VI G ?2 k 1=3 semiconductors. me ¼ ðme me Þ : DOS effective mass jj

System

Material

m? e /m0

me /m0

mGe /m0

III–V

AlN GaN InN

0.29a 0.21 0.047

0.30a 0.22 0.039

0.29–0.45 (0.29a) 0.21 0.044

II–VI

BeO MgSe ZnO ZnS CdS CdSe CdTe

a

0.28 0.150 0.127

0.7a 0.3a 0.234 0.28 0.151 0.125 0.11a

0.28 0.152 0.122

Calculated or estimated

zinc-blende- and wurtzite-type semiconductors are shown in Section 6.2.1 of Adachi [1]. The expressions for the hole effective masses in terms of the Luttingers VB parameters g (cubic) and A (hexagonal) have been described in Section 7.3.1 of Adachi [1]. The g and A values for some cubic and wurtzite semiconductors are summarized in Tables 7.5 and 7.6, respectively. Table 7.7 also lists the effective HH and LH band masses, Table 7.3 Electron effective mass in the X (D) and L minima for some cubic group-IV and III–V semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb)

a

Theoretical

mtX/m0

X

L

mlX/m0

mtL/m0

mlL/m0

0.36 0.1905 0.29 0.086a 0.25

1.4 0.9163 1.35 0.89a 0.67

0.130a 0.081 0.075a

1.418a 1.61 1.478a

0.23a 0.204a 0.32a 0.212a 0.19 0.21 0.30a 0.252 0.23 0.33a 0.34a 0.28a

0.94a 1.125a 0.52a 3.67a 1.1 1.50 0.58a 6.9 1.3 1.30a 1.26a 1.32a

0.15a 0.20a

1.32a 1.82a

0.150a 0.0754 0.085 0.13a 0.12a

1.184a 1.9 1.4 1.64a 3.57a

232

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.4 Electron DOS mass mX;L and conductivity mass mX;L in the X and L minima for some cubic e c group-IV and III–V semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

Density-of-states mass mX e /m0

mLe /m0

mX c /m0

mLc /m0

0.73 0.553 0.51a

0.48 0.259 0.39 0.12a 0.32

0.19 0.119 0.11a

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

1.18 0.669 1.01 0.39a 0.72

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb)

0.76a 0.75a 0.78a 1.14a 0.71 0.84 0.78a 1.58 0.85 1.08a 1.09a 0.98a

a

Conductivity mass

0.78 1.05a 0.75a 0.56 0.54 0.76a 0.94a

0.31a 0.28a 0.37a 0.31a 0.26a 0.29 0.36a 0.37 0.32 0.44a 0.45a 0.38a

0.21a 0.28a 0.21a 0.11 0.12 0.19a 0.18a

Theoretical

mHH and mLH, along the [001] and [111] directions for some cubic semiconductors. The DOS HH ðmHH* Þ, averaged LH ðmLH* Þ and SO split-off hole effective masses (mSO) are summarized in Table 7.8. The c-InN g values in Table 7.5 are taken from Fritsch et al. [3].

7.1.3 Interpolation Scheme Let us consider a linear interpolation representation for the composition dependence of the effective mass m(x) for a semiconductor alloy AxB1x (AxB1xC). The simplest linear interpolation scheme is the use of the equation mAB ðxÞ ¼ xmA þ ð1xÞmB

ð7:6Þ

where mA and mB represent the masses of elemental (binary) semiconductors A (AC) and B (BC), respectively. If any material parameter can be given by a specific expression owing to some physical basis, it is natural to consider that the corresponding interpolation scheme may also obey this specific expression. The effective mass representation can then be written as 1 x 1x ¼ þ mAB ðxÞ mA mB

ð7:7Þ

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

233

Table 7.5 Luttingers VB parameter gi for some cubic group-IV, III–V and II–VI semiconductors (in h2/2m0). d ¼ diamond; zb ¼ zinc-blende System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

BN (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

II–VI

MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

a

g1

g2

g3

4.24 4.285 13.38 15.0 2.817

0.82 0.339 4.24 11.5 0.508

1.71 1.446 5.69 8.6 0.860

1.92a 1.73a 3.47a 3.76a 4.15a 2.84a 4.04 7.10 13.3 5.381a 5.33 20.4 36.3 2.62a 2.84a 3.21a 1.77a 3.94 3.96 4.11a 5.51a 4.14 41.28a 25.96a 15.6

0.02a 0.43a 0.06a 0.90a 1.01a 0.82a 0.53 2.02 4.4 2.294a 1.57 8.3 16.1 0.38a 0.43a 0.52a 0.30a 1.00 0.86 0.77a 1.24a 1.09 21.00a 13.69a 9.6

0.56a 0.65a 1.15a 1.42a 1.75a 1.12a 1.26 2.91 5.7 2.508a 2.11 9.1 17.2 0.91a 1.00a 1.15a 0.62a 1.52 1.39 1.53a 2.14a 1.62 20.73a 13.20a 8.6

Calculated or estimated

Similarly, for quaternary semiconductor alloys of types AxB1xCyD1y and AxByC1xyD (ABxCyD1xy) we obtain 1 xy xð1yÞ ð1xÞy ð1xÞð1yÞ ¼ þ þ þ mABCD ðx; yÞ mAC mAD mBC mBD

ð7:8aÞ

1 x y 1xy ¼ þ þ mABCD ðx; yÞ mAD mBD mCD

ð7:8bÞ

234

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.6 Theoretically obtained Luttingers VB parameter Ai for some wurtzite III–V and II–VI semiconductors A1

A2

A3

A4

A5

A6

|A7|

AlN GaN InN

4.15 6.87 9.15

0.39 0.68 0.66

3.76 6.27 8.50

1.61 2.98 4.52

1.76 3.05 4.47

2.07 4.25 5.74

0.10 0.23 0.33

ZnO ZnS CdS CdSe

3.78 4.58 5.92 10.2

0.44 0.53 0.70 0.76

3.45 4.14 5.37 9.53

1.63 2.34 1.82 3.2

1.68 2.34 1.82 3.2

2.23 3.69 1.36 2.31

0.025

System

Material

III–V

II–VI

Justification for Equation (7.7) is supported by the effective-mass transformation of the Schr€ odinger equation "

# h2 r2 X h2 r2 þ U ðrt Þ ! 2m0 2mAB ðxÞ r

ð7:9Þ

Figure 7.1 shows the effective HH band mass mHH as a function of x for AlxGa1xAs. The solid and dashed lines are obtained by introducing the GaAs (x ¼ 0) and AlAs values (x ¼ 1.0) from Table 7.7 into Equations (7.6) and (7.7), respectively. The dotted lines are obtained by introducing the linearly interpolated g values from Table 7.5 into the following equations (see Table 7.7 in Adachi [1]) mHH½001 ðxÞ ¼

1 g1 ðxÞ2g2 ðxÞ

ð7:10aÞ

mHH½111 ðxÞ ¼

1 g1 ðxÞ2g3 ðxÞ

ð7:10bÞ

It can be seen from Figure 7.1 that the dashed (Equation (7.7)) and dotted lines (Equation (7.10)) agree with each other.

7.2 GROUP-IV SEMICONDUCTOR ALLOY 7.2.1 CSi Binary Alloy The lowest CB valleys in diamond and Si are located at the X (D) point in the BZ [1]. Figure 7.2 X (a) plots the X-valley DOS and conductivity masses mX e and mc for CxSi1x. The solid and dashed lines show the linear interpolation results between diamond and Si listed in Table 7.4 using Equations (7.6) and (7.7), respectively. The solid circles also show the effective masses for 3C-SiC (x ¼ 0.5) taken from Table 7.4.

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

235

Table 7.7 HH and LH effective band masses, mHH and mLH, along the [001] and [111] directions for some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

mHH/m0

Material

smLH/m0

[0 0 1]

[1 1 1]

[0 0 1]

[1 1 1]

0.17 0.202 0.0457 0.026a 0.26

0.13 0.139 0.0404 0.031a 0.22

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

0.38 0.277 0.204 0.125 0.56

1.22 0.718 0.500 0.46 0.91

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

0.53b 0.375b 1.15b 0.30b 0.51b 0.47b 0.83b 0.34 0.33 0.22 1.261 0.46 0.26 0.24

1.25b 0.926b 2.33b 0.85b 1.09b 1.54b 1.67b 0.66 0.78 0.53 2.740 0.90 0.45 0.53

0.51b 0.150b 0.39b 0.28b 0.18b 0.16b 0.22b 0.20 0.090 0.045 0.100 0.12 0.027 0.015

0.33b 0.108b 0.33b 0.17b 0.15b 0.13b 0.20b 0.15 0.077 0.040 0.096 0.11 0.026 0.014

II–VI

MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

1.60b 0.54b 0.51b 0.46b 0.85b 0.52 0.45 0.39b 0.33b 0.51 1.39b 0.70b 0.28

2.77b 1.25b 1.19b 1.10b 1.9b 1.11 0.85 0.95b 0.81b 1.11 5.56b 2.27b 0.63

0.35b 0.30b 0.27b 0.24b 0.42b 0.168 0.176 0.18b 0.13b 0.158 0.012b,c 0.019b,c 0.029c

0.31b 0.23b 0.21b 0.18b 0.33b 0.143 0.148 0.14b 0.10b 0.136 0.012b,c 0.019b,c 0.030c

The sign is chosen positive for a normal band structure like that of Ge Calculated or estimated c The sign is chosen positive for a normal band structure like that of CdTe a b

Figure 7.2(b) shows the HH and LH masses mHH and mLH along the [001] and [111] directions for CxSi1x. The solid lines represent the results calculated from Equation (7.6) using the diamond and Si values in Table 7.7. The 3C-SiC (x ¼ 0.5) values are also plotted in Figure 7.2(b). These values are calculated from a set of the Luttingers VB parameters derived by a five-level kp analysis [4]. Note that the HH and LH bands are anisotropic even in the

236

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.8 DOS HH ðmHH* Þ, averaged LH ðmLH* Þ and SO split-off hole effective masses (mSO) for some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende mHH* /m0

mLH* /m0

mSO/m0

0.78 0.528 0.345 0.029b 0.76

0.14 0.157 0.0427 0.19 0.24

0.394a 0.29 0.095 0.041 0.51

BN (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

0.99a

0.37a 0.0800a 0.35a 0.20a 0.16a 0.13 0.21a 0.17 0.083 0.043 0.098 0.11 0.026 0.014

0.52a 0.2220a 0.58a 0.29a 0.30a 0.317a 0.35a 0.34 0.165 0.12 0.186 0.21 0.14 0.10

MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

0.93a 0.88a 0.80a 1.42a 0.82 0.67 0.68a 0.57a 0.82 0.012a,c 0.019a,c 0.030c

System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

II–VI

1.77a 0.63a 0.81a 0.9 1.27a 0.52 0.55 0.37 1.959 0.69 0.36 0.38

0.25a 0.23a 0.20a 0.36a 0.154 0.159 0.15a 0.11a 0.145 2.22a 1.07a 0.38

0.38a 0.35a 0.31a 0.56a 0.24 0.25 0.24a 0.18a 0.24 0.013a,c 0.031a 0.102a

Calculated or estimated The sign is chosen positive for a normal band structure like that of Ge c The sign is chosen positive for a normal band structure like that of CdTe a b

diamond- and zinc-blende-type semiconductors [1]. As can be easily seen from Figure 7.2(b), the anisotropic effect is most pronounced for the HH band, which has a strongly directionallydependent effective mass, with a larger mass along the [111] direction than along the [001] direction. Using the linear interpolation scheme, we can obtain the plausible effective mass values for 3C-SiC. Note, however, that it is very difficult to accurately measure the effective masses in semiconductors. This is especially true for the hole effective masses and also for the k 6¼ 0

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

237

1.2

Al xGa1-xAs

mHH/m0

1.0

[001] direction

0.8 0.6

[111] direction

0.4 0.2

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.1 Effective HH band mass mHH in the [001] and [111] directions as a function of x for AlxGa1xAs. The solid and dashed lines are calculated from Equations (7.6) and (7.7), respectively. The dotted lines are obtained by introducing the linearly interpolated g values in Table 7.5 into Equation (7.10)

(e.g. X and L valleys) electron masses in semiconductors (and even for the k ¼ 0 (G-valley) electron masses in wide band-gap semiconductors).

7.2.2 SiGe Binary Alloy The transition from a Ge-like CB edge (X (D) valley) to a Si-like edge (L valley) was verified by CR to occur between x ¼ 0.115 and 0.19 [5]. In SixGe1x, the CB edge mass ratios are predicted from Table 7.3 to be mlX/mtX ¼ 10.9 þ 9.0x (Ge-like) and mlL/mtL ¼ 4.8 0.1x (Si-like). Fink and Braunstein [5] carried out CR measurements on the CB of SiGe alloy at 891 GHz (337 mm) using an IR laser. The IR laser enabled measurements of the longitudinal and transverse effective masses to within 4 at% of each side of the alloy composition at which the CB edge switches from the [111] to the [001] direction (15 at% Si in Ge). The measured mass 1.4

1.5

(a)

mHH mLH

1.2

1.0 m eX

0.8 0.6

3C-SiC mcX

0.4

0.9 3C-SiC

0.6 [111]

[001]

0.3

0.2 0

(b)

mHH, mLH (1/m0)

m Xe , m Xc (1/m0)

1.2

CxSi1-x

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

X Figure 7.2 (a) X-valley DOS and conductivity masses mX e and mc for CxSi1x. The solid and dashed lines represent the linear interpolation results derived from Equations (7.6) and (7.7), respectively. The solid circles show the effective masses for 3C-SiC (x ¼ 0.5) taken from Table 7.4. (b) Effective HH and LH band masses mHH and mLH in the [001] and [111] directions for CxSi1x. The solid lines represent the linear interpolation results using Equation (7.6)

238

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.2

0.6 L-X (Δ) crossing m eX

0.8 0.6

m Le

0.4

m Xc Ge-like CB

0.2

(b)

0.5 * , m* , m mHH LH SO (1/m0)

1.0 meX(L) , mX(L) (1/m0) c

(a)

0

0.3 0.2 0.1

0.2 0.4 0.6 0.8 1.0 x

m*HH

0.4

m cL

0

SixGe1-x

0 0

mSO m*LH

0.2 0.4 0.6 0.8 1.0 x

Figure 7.3 (a) X- and L-valley DOS and conductivity masses mX;L and mX;L for SixGe1x. (b) DOS HH e c * * ðmHH Þ, averaged LH ðmLH Þ and SO split-off hole effective masses (mSO) for SixGe1x. The solid lines in (a) and (b) are calculated from Equation (7.6). The dashed line in (a) indicates the CB L–X (D) crossing composition xc 0.15

did not appear to change from their values in the pure constituents, although only the transverse mass of the [111], Ge-like minimum could be measured with reliable accuracy. More recent CR measurements on high-mobility 2D electron gas in strained Si0.94Ge0.06 showed an in-plane mass of 0.193m0 [6], in good agreement with the expectations of Table 7.3. The X- and L-valley DOS and conductivity masses mX;L and mX;L for SixGe1x calculated from Equation (7.6) are e c shown in Figure 7.3(a). Experimental hole masses based on CR are available from measurements of 2D samples for pseudomorphic SixGe1x channels on Si [7]. The results gave insight into the complexity of the VB structure. The DOS HH (mHH ), averaged LH (mLH ) and SO split-off hole effective masses (mSO) for SixGe1x calculated from Equation (7.6) using the Si and Ge values in Table 7.8 are shown in Figure 7.3(b).

7.3 III–V SEMICONDUCTOR TERNARY ALLOY 7.3.1 (III, III)–N Alloy Unfortunately, there is no experimental information on the carrier effective masses in III–N alloys. This necessitates the use of some type of interpolation scheme. The G-valley electron mass mGe versus composition x for c- and w-(III, III)–N ternaries are shown in Figure 7.4. Equation (7.6) is used as the linear interpolation expression. The corresponding endpoint binary data are taken from Tables 7.1 and 7.2.

7.3.2 (III, III)P Alloy Figure 7.5 shows the G-valley electron mass mGe for some P-based ternaries. No experimental determinations of the effective masses in AlxGa1xP and AlxIn1xP appear to be available. Therefore, the electron effective masses mGe in Figure 7.5 were obtained from Equation (7.6). The mGe mass in a random Ga0.5In0.5P alloy was determined to be (0.092 0.003)m0 by

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES 0.30

239

0.4

(a) c-(III, III)-N

(b) w-(III, III)-N

0.25

0.15

meΓ /m0

meΓ /m0

0.3

AlxGa1-xN

0.20

AlxIn1-xN

AlxGa1-xN

0.2

AlxIn1-xN

0.10 GaxIn1-xN

GaxIn1-xN

0.1

0.05 0

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.4 G-valley electron effective mass mGe versus x for (a) c- and (b) w-(III, III)–N alloys. The solid lines are calculated from Equation (7.6)

Emanuelsson et al. [8]. This value is somewhat lower than the linearly interpolated value obtained using Equation (7.6), but is in reasonable agreement with that obtained from Equation (7.7). The quadratic least-squares fit of the x ¼ 0.5 and endpoint data gives a bowing parameter of c ¼ 0.01854m0 (heavy solid line, see also Table 7.9). Emanuelsson et al. [8] found the G-valley electron mass in an ordered Ga0.5In0.5P alloy to be (0.088 0.003)m0, which was slightly smaller than the random alloy value (0.092m0).

7.3.3 (III, III)As Alloy (a) AlGaAs An important description of the carrier effective masses in semiconductors was presented by Adachi [9,10] who reviewed many carried out on GaAs, AlAs and AlxGa1xAs. We have already shown in Figure 7.1 the HH masses mHH in the [001] and [111] directions for 0.24 0.21

meΓ /m0

0.18

AlxGa1-xP

0.15 AlxIn1-xP

0.12 0.09 0.06

GaxIn1-xP

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.5 G-valley electron effective mass mGe versus x for (III, III)–P alloys obtained from the linear interpolation scheme in Equation (7.6) (solid lines). The solid circle represents the CR data for a random Ga0.5In0.5P alloy obtained by Emanuelsson et al. [8]. The heavy solid line shows the quadratic least-squares fit of the endpoint binary data and Emanuelssons data (see Table 7.9)

240

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.9 G-valley electron effective mass mGe determined experimentally for some cubic III–V semiconductor alloys Alloy

mGe /m0

Remark

Gax In1xP AlxGa1xAs Alx In1xAs Gax In1xAs Gax In1xSb GaNx As1x GaPx As1x GaAsxSb1x InPx As1x Inx As1xSb Gax In1xPyAs1y /InP (AlxGa1x)0.48In0.52As/InP

0.07927 þ 0.01619x þ 0.01854x2 0.067 þ 0.057x 0.024 þ 0.088x þ 0.012x2 0.024 þ 0.035x þ 0.008x2 0.013 þ 0.016x þ 0.010x2 0.0067 þ 0.047x (x in at%) 0.067 þ 0.047x 0.039 þ 0.014x þ 0.014x2 0.02400 þ 0.05572x 0.013 0.016x þ 0.027x2 0.04084 þ 0.03384y þ 0.00459y2 0.043 þ 0.031x

0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 2 at% 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 y 1.0 0 x 1.0

AlxGa1xAs. The G-, X- and L-valley electron conductivity masses mGe , mcX and mcL for AlxGa1xAs have been plotted in Figure 7.6(a). The solid lines represent the linear interpolation results of Equation (7.6) using the endpoint binary data in Tables 7.1 and 7.4. The solid circles show the experimental mGe data taken from Adachi [10]. The corresponding linear least-squares fit is represented by the heavy solid line (see also Table 7.9). Figure 7.6(b) plots the cyclotron HH and LH masses mHc and mLc in the [001] direction as a function of x for AlxGa1xAs. The experimental data are taken from Adachi [10]. The cyclotron masses mHc and mLc result from averaging the band effective masses in Equation (47) in Hensel and Suzuki [11]. The solid lines in Figure 7.6(b) show the linear interpolation results between AlAs and GaAs using Equation (7.6), while the heavy solid lines represent the results 1.0 m eX

0.6

meΓ /m0

0.10

0.4 mcX

0.08 meΓ

0.06 0.04 0.02

0

0.2 0

0.7 0.6

mHc

0.20

0.5 mLc

0.4 0.3

Γ-X crossing

0.2

AlxGa1-xAs

0.1

0.2 0.4 0.6 0.8 1.0 x

0.25 (b)

0

0.15 0.10

mLc /m0

0.12

0.8

mHc/m0

(a)

meX, mcX (1/m0)

0.14

0.05 [001] direction

0

0 0.2 0.4 0.6 0.8 1.0 x

X Figure 7.6 (a) G- and X-valley electron effective masses mGe , mX e and mc for AlxGa1xAs. The solid lines show the linearly interpolated results using Equation (7.6). The heavy solid line represents the linear least-squares fit (see Table 7.9). The dashed line indicates the CB G–X crossing composition xc 0.4. (b) Cyclotron HH and LH masses mHc and mLc in the [001] direction for AlxGa1xAs. The solid lines show the linear interpolation results using Equation (7.6). The heavy solid lines are obtained by introducing the linearly interpolated g values into Equation (47) of Hensel and Suzuki [11]. The experimental data in (a) and (b) are taken from Adachi [10] (solid circles)

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

241

calculated by introducing the linearly interpolated g values (Equation (7.6)) into Equation (47) of Hensel and Suzuki [11]. (b) AlInAs Matyas and Karoza [12] determined the G-valley electron mass mGe from a plasma resonance minimum in the IR reflectance spectra for bulk AlxIn1xAs alloy. Their results (solid circles), X together with the linearly interpolated mGe , mX e and mc using Equation (7.6) (solid lines) are shown in Figure 7.7 The experimental mGe data for x > 0.08 are considerably larger than the linearly interpolated values. Similarly, Wright et al. [13] obtained from optically detected CR a considerably larger value of mGe ¼ (0.10 0.01)m0 for Al0.48In0.52As grown by MBE on InP. On the other hand, Cury et al. [14] measured a much smaller mass of mGe ¼ 0.069m0 which is only a little lower than the linearly interpolated value obtained using Equation (7.6) (0.072m0). The smaller result is supported by the optically detected CR measurements by Chen et al. [15]. The heavy solid line in Figure 7.7 shows the quadratic least-squares fit of the endpoint and Curys data (see also Table 7.9). 1.0 meX

0.12

0.6

AlxIn1-xAs

0.10 meΓ /m0

0.8

0.4

0.08

0.2

mcX

meX , mcX (1/m0)

0.14

0

0.06

meΓ

0.04 Γ-X crossing

0.02 0

0

0.2

0.4

0.6

0.8

1.0

x X Figure 7.7 G- and X-valley electron effective masses mGe , mX e and mc for AlxIn1xAs. The solid and open circles represent the experimental data taken from Matyas and Karoza [12] and Cury et al. [14], respectively. The solid lines show the linear interpolation results using Equation (7.6). The heavy solid line shows the quadratic least-squares fit of the endpoint binary data and Curys data (see Table 7.9). The dashed line indicates the CB G–X crossing composition xc 0.63

(c) GaInAs The G-valley electron mass mGe in GaxIn1xAs has been measured by a number of authors [16–20]. These results are shown in Figure 7.8(a). The solid and dashed lines represent the linear interpolation results of Equations (7.6) and (7.7) using the endpoint binary data in Table 7.1, respectively. The heavy solid line shows the quadratic least-squares fit of the experimental data, yielding a small bowing value of c ¼ 0.008m0 (Table 7.9). A set of the Luttingers VB parameters g for GaxIn1xAs have been measured by several authors [21–23]. Traynor et al. [23] observed a significant bowing in k defined by 1 2 2 k ¼ g1 þ g2 þ g3 3 3 3

ð7:11Þ

242

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.08 0.07

8 Gax In1-x As

(a)

6

κ (ħ2/2m0)

meΓ/m0

0.06 0.05 0.04 0.03

5 4 3 2

0.02 0.01 0

(b)

7

1 0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.8 (a) G-valley electron effective mass mGe for GaxIn1xAs. The solid and dashed lines show the linear interpolation results of Equations (7.6) and (7.7), respectively. The heavy solid line represents the quadratic least-squares fit (see Table 7.9). (b) Plots of k values for GaxIn1xAs. The symbols represent the experimental data taken from various sources (see text). The solid and dashed lines are obtained by introducing the linearly interpolated g values of Equations (7.6) and (7.7) into Equation (7.11), respectively

which is a parameter introduced by Luttinger and necessary to describe the magnetic levels, although it is not measured in classical CR experiments. The k values reported by Traynor et al. [23] are plotted against x ¼ 0.08 and 0.11 in Figure 7.8(b) (open triangles), together with those obtained from the Luttingers VB parameters by Alavi et al. [21] for x ¼ 0.47 (solid circle) and Warburton et al. [22] for x ¼ 0.82 (open circle). The solid and dashed lines in Figure 7.8(b) show the k values obtained by introducing the linearly interpolated g values from Equations (7.6) and (7.7) into Equation (7.11), respectively.

7.3.4 (III, III)Sb Alloy No experimental data are available for the effective masses in AlxGa1xSb and AlxIn1xSb. It can be expect however, that the G-valley mass mGe will be satisfactorily represented by the linear interpolation scheme. That is, any nonlinearity in the composition dependence of the effective mass stems entirely from the bowing of the energy band gap (see Figure 7.26). Very little strong bowing in the E0 gap has been observed experimentally for AlxGa1xSb and AlxIn1xSb (Figures 6.25 and 6.26). Figure 7.9(a) shows the G-valley electron mass mGe in GaxIn1xSb measured by Aubin et al. [24]. The solid and dashed lines are obtained by introducing the InSb (x ¼ 0) and GaSb values (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. The heavy solid line represents the quadratic least-squares fit of the experimental data. The VB structure of GaxIn1xSb was investigated by Roth and Fortin [25] using an interband magneto-optical technique. All the fundamental band parameters obtained by these authors exhibited a nonlinear dependence on x. The HH and LH band masses mHH and mLH in the [001] direction for GaxIn1xSb have been plotted in Figure 7.9(b) as examples. These plots are obtained by introducing the nonlinear g values into the expressions shown in Table 7.7 of Adachi [1] (see also an expression for mHH in Equation (7.10a)). The results can be expressed as

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES 0.045 GaxIn1-xSb

0.05

0.5

0.04

[001] direction

0.4

0.030

m HH/m0

meΓ/m0

0.035

0.025

0.015 0.010 0

0.02

mHH

0.2

0.020

0.03

mLH

0.3

0.01

0.1 (a)

0.2 0.4 0.6 0.8 1.0 x

mLH/m0

0.040

0.6

243

(b)

0

0

0 0.2 0.4 0.6 0.8 1.0 x

Figure 7.9 (a) G-valley electron effective mass mGe in GaxIn1xSb. The experimental data are taken from Aubin et al. [24]. The solid and dashed lines are obtained from Equations (7.6) and (7.7), respectively. The heavy solid line shows the quadratic least-squares fit (see Table 7.9). (b) Effective HH and LH band masses mHH and mLH in the [001] direction for GaxIn1xSb. These plots are obtained by introducing the Luttingers VB parameters g determined experimentally by Roth and Fortin [25] into the expressions in Table 7.7 of Adachi [1] (see also Equation (7.12))

mHH ¼ 0:246 m0

ð7:12aÞ

mLH ðxÞ ¼ 0:017 þ 0:009x þ 0:015x2 m0

ð7:12bÞ

7.3.5 Dilute-nitride III–(V, V) Alloy (a) Ga(N, V) alloy The conductivity masses at the lowest direct and indirect conduction minima of GaP are mGe ¼ 0.114m0 (Table 7.1) and mXc ¼ 0.37m0 (Table 7.4), respectively. A large CB effective mass of 0.9m0 has been estimated by analyzing PL spectra for GaNxP1x/GaP MQWs of various well thicknesses [26]. The results may indicate a mixing of the G- and X-valley wavefunctions in the CB. The electron effective mass in dilute-nitride GaNxAs1x has been measured using various techniques, such as optically detected CR [27], PR [28] and magneto-PL measurements [29–31]. These results have been plotted in Figure 7.10. Since the band structure of dilute nitrides is still unclear, let us use a new symbol m*e for the free-electron effective mass. There is a large scatter in m*e . The solid line represents the linear least-squares fit of these data (see also Table 7.9). Zhang and Mascarenhas [32] investigated quantum-confinement phenomena in GaNxAs1x/GaAs QWs (0.009 x 0.045) using an ER technique. They demonstrated formation of an impurity band due to heavy N doping and the quantum confinement of an electron belonging to such an impurity band. The resulting electron effective masses are much larger than those shown in Figure 7.10 (e.g. m*e 0.55m0 at x ¼ 0.009 and 0.4m0 at x ¼ 0.023). The extremely large m*e value with N incorporation and its subsequent decrease can be expected to be a result of the impurity band formation.

244

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.30 0.25

GaNxAs1-x

0.08

0.15 meΓ/m0

meΓ/m0

0.20

0.10 0.05 0 0

0.06 0.04 0.02 0

1

2 x (at%)

3

0.2 0.4 0.6 x (at%)

4

Figure 7.10 Electron effective mass m*e in dilute-nitride GaNxAs1x. The solid line represents the linear least-squares fit (see Table 7.9). The inset shows the experimental results of Young et al. [33] for x from 0 up to 0.4 at%. The solid line in the inset also shows the quadratic least-squares fit of Equation (7.13)

In contrast, by analyzing carrier transport properties Young et al. [33] observed a decrease in m*e with increasing x from 0 up to 0.4 at% in GaNxAs1x. Their results are reproduced in the inset of Figure 7.10. The solid line shows the quadratic least-squares fit of these data (x in at%) m*ðxÞ e ¼ 0:0670:194x þ 0:246x2 m0

ð7:13Þ

The traditional kp theory predicts that the CB mass should decrease with decreasing bandgap energy [1] (Figure 7.26). We have shown that adding N to GaAs reduces its band-gap energy considerably (Figure 6.29), so this effect alone may be expected to reduce the effective mass. On the other hand, any effect of N incorporation on the CB wavefunction admixture will increase the electron effective mass [34]. Young et al. [33] considered that their samples lay at the limit of dilute alloy where there are minor perturbations of the CB. The observed m*e reduction is thus thought to be due to the band-gap reduction. The large increase in m*e observed in the intermediate or higher N concentration region [27–31] is due to the mixing effect of the CB states (G, X and L). The effect of N incorporation on the electron effective mass is more subtle and it may represent a more stringent test for the validity of different theoretical models aimed at explaining the puzzling effects of N in various III–V semiconductors [34]. Unfortunately, the experimental m*e data reported do not show a common and clear trend with increasing N concentration, as can be seen from Figure 7.10. (b) In(N, V) alloy The electron effective mass m*e in dilute-nitride InNxAs1x has been measured by several authors [35–37]. Figure 7.11 plots the results obtained by these authors (solid circles: Huang et al. [35]; open circle: Hang et al. [36]; open triangles: Shih et al. [37]). The heavy solid line shows the quadratic least-squares fit of these data (x in at%)

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

245

0.4

meΓ/m0

0.3

InNx As1-x

0.2 0.1 0 0

1

2

3

4

x (at%)

Figure 7.11 Electron effective mass m*e in dilute-nitride InNxAs1x. The solid and dashed lines are calculated by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. Note that these lines completely overlap in the region of x 4 at%. The heavy solid line shows the quadratic least-squares fit of Equation (7.14)

m*e ðxÞ ¼ 0:0240:018x þ 0:029x2 m0

ð7:14Þ

The solid and dashed lines are obtained by introducing the InAs (x ¼ 0) and c-InN values (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. The effective mass m*e in dilute-nitride InNxSb1x has been measured by Murdin et al. [38] using the CR technique. The experimental m*e value for x ¼ 0.044 at 5.53 mm exciting laser wavelength was 0.044, which was compared with 0.033 for InSb (x ¼ 0) at the same wavelength. Since N incorporation mainly affects the CB states [34], the dilute-nitride hole effective masses can be compared with those of the hole masses in the nitride-free III–V host semiconductors, such as GaP, GaAs, InAs and InSb.

7.3.6 Al(V, V) Alloy No experimental data are available on the effective masses of Al-based ternary alloys. Therefore, the linearly interpolated mGe values for AlPxAs1x, AlPxSb1x and AlAsxSb1x using Equation (7.6) are shown in Figure 7.12. The endpoint binary masses are taken from Table 7.1.

7.3.7 Ga(V, V) Alloy (a) GaPAs Figure 7.13(a) shows the G-valley electron effective mass mGe in GaPxAs1x measured by Wetzer et al. [39] using an optical detection CR technique. The solid and dashed lines represent the linear interpolation results obtained by introducing the GaAs (x ¼ 0) and GaP values (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. There is a tendency for upward bowing in the experimental mGe versus x plots; however, the same alloy showed a weak downward bowing in E0 (Figure 6.33). It can, therefore, be concluded that GaPxAs1x has an almost linear dependence of mGe on x. The resulting expression is given in Table 7.9.

246

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.24 0.21 meΓ/m0

0.18

AlPxAs1-x AlPxSb1-x

0.15 0.12

AlAsxSb1-x

0.09 0.06

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.12 G-valley electron effective mass mGe versus x for Al(V, V) alloys obtained from the linear interpolation scheme of Equation (7.6)

(b) GaAsSb Filion and Fortin [40] determined the G-valley electron effective mass mGe in GaAsxSb1x by measuring intrinsic photoconductivity under magnetic fields of up to 65 kG. The data they obtained for mGe , together with the linearly interpolated results using Equations (7.6) and (7.7) are shown in Figure 7.13(b). The result calculated using Equation (7.7), shown by the dashed line, explains the peculiar experimental data very well and can be approximated by the quadratic expression given in Table 7.9.

7.3.8 In(V, V) Alloy (a) InPAs The electron effective mass mGe in InPxAs1x has been measured by various authors [41–45]. The solid line in Figure 7.14 represents the linear least-squares fit of these data (see Table 7.9). 0.14

0.08 (a) GaPxAs1-x

(b) GaAsxSb1-x

0.07

0.12

meΓ/m0

meΓ/m0

0.06 0.10 0.08

0.05 0.04

0.06 0.04 0

0.03 0.2 0.4 0.6 0.8 1.0 x

0.02

0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.13 G-valley electron effective mass mGe versus x for (a) GaPxAs1x and (b) GaAsxSb1x. The experimental data in (a) are taken from Wetzel et al. [39] and in (b) from Filion and Fortin [40] (solid circles). The solid and dashed lines are obtained by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. The expressions used to obtain these lines are listed in Table 7.9

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

247

0.10

meΓ/m0

0.08

InPxAs1-x

0.06 0.04 0.02 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.14 G-valley electron effective mass mGe in InPxAs1x. The solid line represents the linear least-squares fit (see Table 7.9)

(b) InAsSb The electron effective mass mGe in InAsxSb1x obtained from Thomas and Woolley [46] is shown in Figure 7.15(a). The solid and dashed lines represent the linear interpolation results obtained by introducing the InSb (x ¼ 0) and InAs data (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. The heavy solid line also shows the quadratic least-squares fit of the experimental data. The bowing parameter c obtained from this fit is 0.027m0, which is much larger than the endpoint values mGe ¼ 0.013m0 (InSb) and 0.024m0 (InAs). The resulting mGe versus x curve exhibits considerably large downward bowing, as shown in Figure 7.15(a). A full set of the Luttingers VB parameters for InAsxSb1x have been determined by Smith et al. [47] from interband magnetoabsorption measurements. The results they obtained have been plotted in Figure 7.15(b). These parameters show almost linear dependence on x.

0.030

40 Inx As1-xSb

32

0.020

γi (ħ2/2m0)

meΓ/m0

(b)

36

(a)

0.025

0.015

28

γ1

24 20 16

0.010

γ2

12 0.005 0

0.2 0.4 0.6 0.8 1.0 x

8

0

γ3

0.2 0.4 0.6 0.8 1.0 x

Figure 7.15 (a) G-valley electron effective mass mGe in InAsxSb1x. The experimental data are taken from Thomas and Woolley [46]. The solid and dashed lines are obtained by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. The heavy solid line shows the quadratic leastsquares fit (see Table 7.9). (b) Luttingers VB parameters for InAsxSb1x determined by Smith et al. [47]

248

PROPERTIES OF SEMICONDUCTOR ALLOYS

7.4 III–V SEMICONDUCTOR QUATERNARY ALLOY 7.4.1 Dilute-nitride Quaternary Alloy As mentioned in Section 7.3.5, the electron effective mass m*e in dilute-nitride III–V ternaries is usually larger than the electron effective mass mGe in the host materials, possibly due to the interaction of the CB with N-related resonant states. The same conclusion can be drawn for dilutenitride III–V quaternaries. The electron effective mass m*e in dilute-nitride GaxIn1xNyAs1y obtained by Pan et al. [48] and Heroux et al. [49] is shown in Figure 7.16. These data show a clear increase in m*e with increasing N concentration. A number of groups also observed an increase in the electron effective mass by incorporating N atoms into GaxIn1xAs [50–54]. 0.12

GaxIn1-xNyAs1-y me*/m0

0.10 0.08 0.06 0.04

x=0.7 0.86 0

0.5

1.0

1.5

2.0

N (at%)

Figure 7.16 Electron effective mass m*e in dilute-nitride GaxIn1xNyAs1y reported by Pan et al. [48] (solid circles) and Herouz et al. [49] (open circles)

Polimeni et al. [55] found that there was dependence of the in-plane hole effective masses in GaxIn1xNyAs1y QWs on the In concentration by PL measurements after picosecond excitation and under a magnetic field B. These results suggest that the dilute-nitride hole effective masses are nearly the same as those for nitride-free GaxIn1xAs host semiconductor. This agrees with the fact that N incorporation mainly affects the CB states [34].

7.4.2 (III, III)–(V, V) Alloy (a) GaInPAs Adachi [56] has reviewed the carrier effective masses in GaxIn1xPyAs1y. The G-valley electron effective mass mGe versus y for GaxIn1xPyAs1y/InP has been plotted in Figure 7.17(a). The solid and dashed lines represent the linear interpolation results obtained from Equations (A.6) and (7.8) respectively, using the binary data in Table 7.1. The solid circles show the experimental data taken from Adachi [56]. The corresponding quadratic least-squares fit is given by the heavy solid line (see also Table 7.9). The LH effective mass in GaxIn1xPyAs1y/InP versus y is plotted in Figure 7.17(b). The experimental data are taken from Adachi [56]. The solid and dashed lines represent the linear interpolation results obtained from Equations (A.6) and (7.8) respectively, using the binary data in Table 7.7. The heavy solid line shows the quadratic best-fit expression

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES 0.10

249

0.14 GaxIn1-xPyAs1-y /InP

0.12

0.08 mLH /m0

meΓ/m0

0.10 0.06

0.08 0.06

0.04 0.04

(a) 0.02 0

(b)

0.2 0.4 0.6 0.8 1.0 y

0.02 0

0.2 0.4 0.6 0.8 1.0 y

Figure 7.17 (a) G-valley electron effective mass mGe and (b) LH effective mass mLH versus y for GaxIn1xPyAs1y /InP. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively. The solid circles show the experimental data taken from Adachi [56]. The heavy solid lines represent the quadratic least-squares fit in Table 7.9 ðmGe Þ and the result obtained using Equation (7.15) (mLH). The open squares correspond to the InP (y ¼ 1.0) data

mLH ðyÞ ¼ 0:05 þ 0:04y þ 0:03y2 m0

ð7:15Þ

(b) GaInAsSb No experimental data on the carrier effective masses in GaxIn1xAsySb1y has been reported. The linearly interpolated mGe values for GaxIn1xAsySb1y lattice-matched to GaSb and InAs have therefore been plotted in Figure 7.18. The solid and dashed lines represent the linear interpolation results of Equations (A.6) and (7.8) respectively, using the binary data in 0.05

0.05

(a)

(b) 0.04 meΓ/m0

meΓ/m0

0.04

0.03

0.02

0.03

0.02 GaxIn1-xAsySb1-y /GaSb

0.01 0

0.2 0.4 0.6 0.8 1.0 x

Gax In1-x AsySb1-y /InAs

0.01 0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.18 G-valley electron effective mass mGe versus x for (a) GaxIn1xAsySb1y /GaSb and (b) GaxIn1xAsySb1y/InAs. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively

250

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.1. The results of GaxIn1xPyAs1y / InP in Figure 7.17 support the use of Equation (A.6) for providing more plausible effective masses for III–V semiconductor alloys.

7.4.3 (III, III, III)–V Alloy (a) AlGaInP The electron effective mass mGe in (AlxGa1x)0.53In0.47P/GaAs has been measured by Emanuelsson et al. [8] using conventional and optically detected CR measurements. The result they obtained mGe /m0 ¼ 0.14 0.01 (x ¼ 0.3) is shown in Figure 7.19, together with those calculated from Equations (A.6) and (7.8) using the binary data in Table 7.1 (solid and dashed lines). The experimental data is found to be slightly larger than the interpolated value obtained using Equation (A.6) (solid line). This may be due to X-valley interactions (see Figure 6.49) and/or any effect of band nonparabolicity.

Figure 7.19 G-valley electron effective mass mGe versus x for (AlxGa1x)0.53In0.47P/GaAs. The solid circle represents the experimental data taken from Emanuelsson et al. [8]. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively

(b) AlGaInAs The G-valley electron effective mass mGe in (AlxGa1x)0.48In0.52As/InP has been measured by several authors [14,15,57,58]. Figure 7.20 shows these results (solid circles), together with those obtained from Equations (A.6) and (7.8) using the binary data in Table 7.1 (solid and dashed lines). The linear least-squares fit of the experimental data is also shown by the heavy solid line (see also Table 7.9). Equation (A.6) has been found to estimate mGe more reliably than Equation (7.8).

7.4.4 III–(V, V, V) Alloy Theelectron effective mass mGe in InPxAsySb1xy/InAs hasbeen measured byVoronina et al. [59] using various techniques, such as the Shubnikov–de Haas effect, Hall effect, magnetoresistance and photoconductivity. This result is plotted in Figure 7.21 (x ¼ 0.26, y ¼ 0.62). The solid and dashed lines show the linear interpolation results of Equations (A.6) and (7.8) respectively, using the binary data in Table 7.1. It can be seen that the experimental data is slightly smaller than the linearly interpolated value derived using Equation (A.6) (solid line).

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

251

0.09 (AlxGa1-x)0.48In0.52As/InP

0.08 meΓ /m0

0.07 0.06 0.05 0.04 0.03

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.20 G-valley electron effective mass mGe versus x for (AlxGa1x)0.48In0.52As/InP. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively. The heavy solid line shows the quadratic least-squares fit (see Table 7.9)

0.08

InPx AsySb1-x-y /InAs meΓ /m0

0.06 0.04 0.02 0

0

0.2

0.4

0.6

0.8

1.0

y

Figure 7.21 G-valley electron effective mass mGe versus x for InPxAsySb1xy/InAs. The solid circle represents the experimental data taken from Voronina et al. [59]. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively

7.5 II–VI SEMICONDUCTOR ALLOY 7.5.1 (II, II)–VI Ternary Alloy Lu et al. [60] obtained the electron effective mass mGe in MgxZn1xO from analyzing the Burstein–Moss shift. The mass values they obtained are plotted in Figure 7.22(a). The electron effective mass increased with increasing x from 0.30m0 (x ¼ 0) to 0.49m0 (x ¼ 0.21). Note, however, that the ZnO (x ¼ 0) value is slightly larger than that estimated from the generalized mGe versus E0 relationship (0.23m0) [1]. Figure 7.22(b) shows the G-valley electron effective mass mGe in c-ZnxCd1xSe reported by Imanaka and Miura [61] (solid circle), Lo et al. [62] (open circle) and Ng et al. [63] (open triangles). We can see that the data of Lo et al. is considerably larger than that estimated from the linear interpolation scheme (solid and dashed lines). Shao et al. [64] also determined the mGe value in Zn0.80Cd0.20Se/ZnS0.06Se0.94 QW by Shubnikov–de Haas oscillations. The

252

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.8

0.16 (a) MgxZn1-xO

0.7

0.15

(b) c-ZnxCd1-xSe

wurtzite

0.14 rocksalt

0.5

meΓ/m0

meΓ/m0

0.6

0.4

0.13 0.12

mixed phase

0.3 0.2 0

0.11 0.10 0

0.2 0.4 0.6 0.8 1.0 x

0.2 0.4 0.6 0.8 1.0 x

Figure 7.22 (a) G-valley electron effective mass mGe in MgxZn1xO. The experimental data are taken from Lu et al. [60]. (b) G-valley electron effective mass mGe in c-ZnxCd1xSe. The experimental data are taken from Imanaka and Miura [61] (solid circle), Lo et al. [62] (open circle) and Ng et al. [63] (open triangles). The solid and dashed lines in (b) are obtained by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. The open squares in (a) and (b) show the endpoint binary data in Table 7.1

value they obtained, 0.17m0 (x ¼ 0.80) is, however, much larger than the endpoint binary data. The larger mGe value was considered to be due to the effect of a parallel conduction layer in the sample measured [64]. The Hg-based ternaries ZnxHg1xTe and CdxHg1xTe exhibit a semimetallic nature at low x compositions (E0 < 0 eV, see Figure 6.58). The corresponding CB electrons have a negative mass value. The G-valley electron effective masses mGe in ZnxHg1xTe and CdxHg1xTe are shown in Figure 7.23. The experimental data for ZnxHg1xTe are taken from Shneider and Tsiutsiura [65] and for CdxHg1xTe from Kim and Narita [66] (open triangles) and Laurenti 0.20

0.10 (a) ZnxHg1-xTe

0.15

0.08 0.06 meΓ/m0

meΓ/m0

0.10 0.05 0

T= 0 K 300 K

0.04 0.02 0

semimetallic

-0.05 -0.10

(b) CdxHg1-xTe

0

0.2 0.4 0.6 0.8 1.0 x

-0.02 -0.04 0

semimettalic

0.2 0.4 0.6 0.8 1.0

Figure 7.23 G-valley electron effective mass mGe in (a) ZnxHg1xTe and (b) CdxHg1xTe. The experimental data in (a) are taken from Shneider and Tsiutsiura [65] and in (b) from Kim and Narita [66] (at 4.2 K, open triangles) and Laurenti et al. [67] (at 0 K (solid circles) and 300 K (open circles)). The solid lines in (a) and (b) are obtained by introducing the endpoint binary data into Equation (7.6)

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

253

et al. [67] (T ¼ 0 K (solid circles), 300 K (open circles)). A large difference can be seen between the experimental and linearly interpolated values for ZnxHg1xTe. Note that the Hg-based alloys have positive and strongly x-dependent coefficients dE0/dT at high Hg concentrations (Figure 6.57). The semimetal/semiconductor crossing composition and free-electron concentration then show strong temperature dependence [67–69]. These facts make it difficult to accurately determine the electron effective mass at high Hg concentration. Note also that the lowest CB minimum in a semiconductor region is at the G6 state while that in a semimetal region is at the G8 state (i.e. the LH band in the cubic, zinc-blende semiconductors).

7.5.2 II–(VI, VI) Ternary Alloy The G-valley electron effective mass mGe in w-CdSxSe1x has been determined by analyzing optical absorption spectra using a kp method [70]. These results have been plotted in Figure 7.24. The solid line also shows the linear interpolation result obtained by introducing the endpoint binary data in Table 7.1 into Equation (7.6). 0.30

w-CdSxSe1-x

meΓ/m0

0.24 0.18 0.12 0.06 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.24 G-valley electron effective mass mGe in w-CdSxSe1x. The experimental data are taken from Brodin et al. [70]. The solid line is obtained by introducing the endpoint binary data into Equation (7.6)

Brodin et al. [70] reported the x-dependent hole effective masses at the three VB states (G9, G7 and G7). All these hole masses and mGe (Figure 7.24) increased almost linearly from CdSe (x ¼ 0) to CdS (x ¼ 1.0).

7.5.3 (II, II)–(VI, VI) Quaternary Alloy No detailed experimental determinations of the electron or hole effective mass in II–VI quaternary alloys have been carried out. Therefore, the G-valley electron effective mass mGe in MgxZn1xSySe1y/GaAs obtained from the linear interpolation scheme is shown in Figure 7.25. The solid and dashed lines were obtained from Equations (A.6) and (7.8), respectively. The interpolated values show upward bowing. For example, the solid line can be expressed as mGe ðxÞ ¼ 0:14 þ 0:12x0:04x2 m0

ð7:16Þ

254

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.30

Mgx Zn1-xSySe1-y /GaAs

meΓ/m0

0.25 0.20 0.15 0.10

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.25 G-valley electron effective mass mGe in MgxZn1xSySe1y/GaAs. The solid and dashed lines are calculated by introducing the binary data into Equations (A.6) and (7.8), respectively

7.6 CONCLUDING REMARKS 7.6.1 Composition Dependence The simple three-band kp theory gives m0 P2 2 1 P2 P2 0 ¼ 1 þ þ þ C / þ C

mGe 3 E0 E0 þ D0 E0 E0

ð7:17Þ

where P is the momentum matrix element relating the p-like VB to the s-like CB and C (C 0 ) is a correction for all higher-lying bands. Thus, the G-valley electron effective mass mGe is expected to be proportional to E0 (see Equations (7.8) and (7.9) in Adachi [1]). Figure 7.26 plots the E0 and mGe versus x for some cubic III–V ternaries. It can be seen that the smaller E0-gap material has a smaller mGe value, as predicted by Equation (7.17). The results in Sections 7.2–7.5 also indicate that linear interpolation (especially Equation (7.6) or Equation (A.6)) is an easy and effective means to obtain the electron and hole effective masses in semiconductor alloys.

7.6.2 External Perturbation Effect Like the G-point energy gaps (E0 and E0 þ D0 ), the electron and hole effective masses at the G point of non-alloyed semiconductors decrease with increasing temperature (T) and also increase with increasing pressure p [1]. The same tendency can be expected in semiconductor alloys. Laurenti et al. [67] observed that increasing T from 0 to 500 K leads to a gradual decrease in the mGe value of CdxHg1xTe for x 0.5. Similarly, Nicholas et al. [42] found that for InPxAs1x (0 x 1.0) the value of mGe was relatively constant from low T up to T 100 K and that further increases in T decreased mGe in an almost proportional manner. The change in the electron effective mass DmGe from T ¼ 0 to 300 K was less than 8%. The pressure dependence of the electron effective mass mGe in InPxAs1x has been measured by Torres and Stradling [44]. These results have been plotted in Figure 7.27. It can be seen that mGe increases almost linearly with increasing p. Similarly, an increase in mGe has been observed in Ga0.47In0.53As [71,72] and also in dilute-nitride GaxIn1xNyAs1y (m*e ) [73,74].

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

255

3.5 (a)

3.0

E0 (eV)

2.5 2.0 1.5 1.0 0.5 0 0.15 (b)

meΓ/m0

0.10

0.05

0 AlAs

GaAs

InAs x

InSb

GaSb

Figure 7.26 (a) Lowest direct gap (E0) at 300 K and (b) G-valley electron effective mass ðmGe Þ versus composition x for some III–V ternaries. The experimental data are plotted by the solid circles

6.4 InPx As1-x

meΓ /m×0 (x10-2)

6.0

x = 0.66

5.6 4.8 x = 0.31

4.4 4.0

x = 0.22

3.6 0

0.4

0.8

1.2

1.6

p (GPa)

Figure 7.27 Pressure dependence of mGe in InPxAs1x. The experimental data are taken from Torres and Stradling [44]

PROPERTIES OF SEMICONDUCTOR ALLOYS

meΓ/m0

meΓ/m0

256

0.16 0.14 (a) GaxIn1-xAs 0.12 x = 0.22 ( ) 0.34 0.10 0.47 0.08 0.06 0.04 18 10 1019 0.18 0.16 (b) InP xAs1-x 0.14 x = 0.29 0.12 0.48 ( ) 0.69 0.10 0.08 0.06 0.04 18 10 1019 n (cm-3)

1020

1020

Figure 7.28 Free-electron concentration dependence of mGe in (a) GaxIn1xAs and (b) InPxAs1x. The experimental data are taken from Metzger et al. [75]. The solid lines show the least-squares fits given by (a) ln(mGe /m0) ¼ (2.24 1020)n 2.89 (x ¼ 0.22) and (b) ln(mGe /m0) ¼ (2.04 1020)n 2.95 (x ¼ 0.48) with n in cm3, respectively

The highest VBs and lowest CB of III–Vand II–VI semiconductors are nonparabolic. Since the band nonparabolicity becomes significant as the Fermi level moves deep in the band, the electron effective mass in semiconductors increases with doping level for carrier concentrations larger than 1018 cm3. The dependence of the electron effective mass mGe on electron concentration in GaxIn1xAs and InPxAs1x has been reported by Metzger et al. [75]. Their results are reproduced in Figure 7.28. The electron effective masses increase abruptly as a function of free-electron density and converge at n 5 1019 cm3. They concluded that the Kanes band model offers an accurate description of CB nonparabolicity. An increase in m*e with increasing free-electron density has also been observed in dilute-nitride GaxIn1xNyAs1y [74].

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] T. Hofmann, T. Chavdarov, V. Darakchieva, H. Lu, W. J. Schaff, and M. Schubert, Phys. Status Solidi C 3, 1854 (2006). [3] D. Fritsch, H. Schmidt, and M. Grundmann, Phys. Rev. B 69, 165204 (2004). [4] D. Bimberg, M. Altarelli, and N. O. Lipari, Solid State Commun. 40, 437 (1981). [5] D. Fink and R. Braunstein, Phys. Status Solidi B 73, 361 (1976). [6] C. W. Liu and V. Venkataraman, Mater. Chem. Phys. 49, 29 (1997). [7] J. F. N€utzel, C. M. Engelhardt, and G. Abstreiter, in Properties of Strained and Relaxed Silicon Germanium, EMIS Datareviews Series No. 12 (edited by E. Kasper), INSPEC, London, 1995, p. 103. [8] P. Emanuelsson, M. Drechsler, D. M. Hofmann, and B. K. Meyer, Appl. Phys. Lett. 64, 2849 (1994). [9] S. Adachi, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, pp. 58–72.

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

257

[10] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [11] J. C. Hensel and K. Suzuki, Phys. Rev. B 9, 4219 (1974). [12] E. E. Matyas and A. G. Karoza, Phys. Status Solidi B 111, K45 (1982). [13] M. G. Wright, A. Kanaah, B. C. Cavenett, G. R. Johnson, and S. T. Davey, Semicond. Sci. Technol. 4, 590 (1989). [14] L. A. Cury, J. Beerens, and J. P. Praseuth, Appl. Phys. Lett. 63, 1804 (1993). [15] Y. F. Chen, Y. T. Dai, J. C. Fan, T. L. Lee, and H. H. Lin, Appl. Phys. Lett. 67, 1256 (1995). [16] M. B. Thomas and J. C. Woolley, Can. J. Phys. 49, 2052 (1971). [17] H. Fetterman, J. Waldman, and C. M. Wolfe, Solid State Commun. 11, 375 (1972). [18] C. K. Sarkar, R. J. Nicholas, J. C. Portal, M. Razeghi, J. Chevrier, and J. Massies, J. Phys. C: Solid State Phys. 18, 2667 (1985). [19] Y. T. Dai, J. L. Shen, Y. F. Chen, S. Z. Chang, and S. C. Lee, Chin. J. Phys. 36, 20 (1998). [20] J. L. Shen, Y. D. Dai, Y. F. Chen, S. Z. Chang, and S. C. Lee, Phys. Rev. B 51, 17648 (1995). [21] K. Alavi, R. L. Aggarwal, and S. H. Groves, Phys. Rev. B 21, 1311 (1980). [22] R. J. Warburton, R. W. Martin, R. J. Nicholas, L. K. Howard, and M. T. Emeny, Semicond. Sci. Technol. 6, 359 (1991). [23] N. J. Traynor, R. J. Warburton, M. J. Snelling, and R. T. Harley, Phys. Rev. B 55, 15701 (1997). [24] M. J. Aubin, M. B. Thomas, E. H. van Tongerloo, and J. C. Woolley, Can. J. Phys. 47, 631 (1969). [25] A. P. Roth and E. Fortin, Can. J. Phys. 56, 1468 (1978). [26] H. P. Xin and C. W. Tu, Appl. Phys. Lett. 77, 2180 (2000). [27] P. N. Hai, W. M. Chen, I. A. Buyanova, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 77, 1843 (2000). [28] J. Wu, W. Shan, W. Walukiewicz, K. M. Yu, J. W. Ager III, E. E. Haller, H. P. Xin, and C. W. Tu, Phys. Rev. B 64, 085320 (2001). [29] Y. J. Wang, X. Wei, Y. Zhang, A. Mascarenhas, H. P. Xin, Y. G. Hong, and C. W. Tu, Appl. Phys. Lett. 82, 4453 (2003). [30] F. Masia, A. Polimeni, G. B. H. von H€ogersthal, M. Bissiri, P. J. Klar, and W. Stolz, Appl. Phys. Lett. 82, 4474 (2003). [31] F. Masia, G. Pettinari, A. Polimeni, M. Felici, A. Miriametro, M. Capizzi, A. Lindsay, S. B. Healy, E. P. OReilly, A. Cristofoli, G. Bais, M. Piccin, S. Rubini, F. Martelli, A. Faranciosi, P. J. Klar, K. Volz, and W. Stolz, Phys. Rev. B 73, 073201 (2006). [32] Y. Zhang and A. Mascarenhas, Phys. Rev. B 61, 7479 (2000). [33] D. L. Young, J. F. Geisz, and T. J. Coutts, Appl. Phys. Lett. 82, 1236 (2003). [34] See, for example, M. Henini, Dilute Nitride Semiconductors, Elsevier, Amsterdam, 2005. [35] W. K. Hung, K. S. Cho, M. Y. Chern, Y. F. Chen, D. K. Shih, H. H. Lin, C. C. Lu, and T. R. Yang, Appl. Phys. Lett. 80, 796 (2002). [36] D. R. Hang, C. F. Huang, W. K. Hung, Y. H. Chang, J. C. Chen, H. C. Yang, Y. F. Chen, D. K. Shih, T. Y. Chu, and H. H. Lin, Semicond. Sci. Technol. 17, 999 (2002). [37] D. -K. Shih, H. -H. Lin, L. -W. Sung, T. -Y. Chu, and T. -R. Yang, Jpn. J. Appl. Phys. 42, 375 (2003). [38] B. N. Murdin, A. R. Adams, P. Murzyn, C. R. Pidgeon, I. V. Bradley, J. -P. R. Wells, Y. H. Matsuda, N. Miura, T. Burke, and A. D. Johnson, Appl. Phys. Lett. 81, 256 (2002). [39] C. Wetzel, B. K. Meyer, and P. Omling, Phys. Rev. B 47, 15588 (1993). [40] A. Filion and E. Fortin, Can. J. Phys. 52, 743 (1974). [41] R. J. Nicholas, R. A. Stradling, and J. C. Ramage, J. Phys. C: Solid State Phys. 12, 1641 (1979). [42] R. J. Nicholas, R. A. Stradling, J. C. Portal, and S. Askenazy, J. Phys. C: Solid State Phys. 12, 1653 (1979). . Rut, Sov. Phys. Semicond. 16, 596 (1982). [43] V. V. Kruzhaev, G. M. Minkov, and O. E [44] C. M. S. Torres and R. A. Stradling, Semicond. Sci. Technol. 2, 323 (1987). [45] T. W. Kim, D. C. Choo, D. U. Lee, M. Jung, and S. O. Kang, J. Phys. Chem. Solids 63, 875 (2002). [46] M. B. Thomas and J. C. Woolley, Can. J. Phys. 49, 2056 (1971).

258

PROPERTIES OF SEMICONDUCTOR ALLOYS

[47] S. N. Smith, C. C. Phillips, R. H. Thomas, R. A. Stradling, I. T. Ferguson, A. G. Norman, B. N. Murdin, and C. R. Pidgeon, Semicond. Sci. Technol. 7, 900 (1992). [48] Z. Pan, L. H. Li, Y. W. Lin, B. Q. Sun, and D. S. Jiang, Appl. Phys. Lett. 78, 2217 (2001). [49] J. B. Herouz, X. Yang, and W. I. Wang, J. Appl. Phys. 92, 4361 (2002). [50] M. Hetterich, M. D. Dawson, A. Y. Egorov, D. Bernkiau, and H. Riechert, Appl. Phys. Lett. 76, 1030 (2000). [51] C. Skierbiszewski, P. Perlin, P. Wisniewski, W. Knap, T. Suski, W. Walukiewicz, W. Shan, K. M. Yu, J. W. Ager, E. E. Haller, J. F. Geisz, and J. M. Olson, Appl. Phys. Lett. 76, 2409 (2000). [52] J. -Y. Duboz, J. A. Gupta, M. Byloss, G. C. Aers, H. C. Liu, and Z. R. Wasilewski, Appl. Phys. Lett. 81, 1836 (2002). [53] C. Skierbiszewski and J. Łusakowski, J. Phys.: Condens. Matter 16, S3319 (2004). [54] M. H. Gass, A. J. Papworth, T. B. Joyce, T. J. Bullough, and P. R. Chalker, Appl. Phys. Lett. 84, 1453 (2004). [55] A. Polimeni, F. Masia, A. Vinattieri, G. B. H. von H€ ogersthal, and M. Capizzi, Appl. Phys. Lett. 84, 2295 (2004). [56] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992. [57] D. Olego, T. Y. Chang, E. Silberg, E. A. Caridi, and A. Pinczuk, Appl. Phys. Lett. 41, 476 (1982). [58] R. F. Kopf, H. P. Wei, A. P. Perley, and G. Livescu, Appl. Phys. Lett. 60, 2386 (1992). [59] T. I. Voronina, T. S. Lagunova, K. D. Moiseev, M. A. Sipovskaya, I. N. Timchenko, and Y. P. Yakovlev, Semicond. 27, 978 (1993). [60] J. G. Lu, S. Fujita, T. Kawaharamura, H. Nishinaka, Y. Kamada, and T. Ohshima, Appl. Phys. Lett. 89, 262107 (2006). [61] Y. Imanaka and N. Miura, Physica B 249–251, 932 (1998). [62] I. Lo, S. J. Chen, L. -W. Tu, W. C. Mitchel, R. C. Tu, and Y. K. Su, Phys. Rev. B 60, R11281 (1999). [63] H. K. Ng, Y. A. Leem, R. Knobel, I. P. Smorchkova, A. A. Sirenko, and N. Samarth, Appl. Phys. Lett. 75, 3662 (1999). [64] H. Shao, S. Scholl, H. Sch€afer, J. Gersch€utz, B. Jobst, D. Hommel, and G. Landwehr, Solid State Commun. 100, 739 (1996). [65] A. D. Shneider and D. I. Tsiutsiura, Phys. Status Solidi A 5, K39. (1971). [66] R. S. Kim and S. Narita, Phys. Status Solidi B 73, 741 (1976). [67] J. P. Laurenti, J. Camassel, A. Bouhemadou, B. Toulouse, R. Legros, and A. Lusson, J. Appl. Phys. 67, 6454 (1990). [68] J. Chu, Z. Mi, and D. Tang, Infrared Phys. 32, 195 (1991). [69] Y. -G. Sha, C. -H. Su, and S. L. Lehoczky, J. Appl. Phys. 81, 2245 (1997). [70] M. S. Brodin, M. V. Kurik, and S. P. Yurtsenyuk, Sov. Phys. Solid State 7, 2516 (1966). [71] D. Gauthier, L. Dmowski, J. C. Portal, D. Leadley, M. A. Hopkins, M. A. Brummell, R. J. Nicholas, M. Razeghi, and P. Maurel, Superlatt. Microstruct. 4, 201 (1988). [72] S. Charlebois, J. Beerens, C. J. Miner, and N. Puetz, Phys. Rev. B 54, 13456 (1996). [73] C. Skierbiszewski, P. Erlin, P. Wisniewski, T. Suski, J. F. Geisz, K. Hingerl, W. Jantsch, D. E. Mars, and W. Walukiewicz, Phys. Rev. B 65, 035207 (2001). [74] C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002). [75] W. K. Metzger, M. W. Wanlass, L. M. Gedvilas, J. C. Verley, J. J. Carapella, and R. K. Ahrenkiel, J. Appl. Phys. 92, 3524 (2002).

8 Deformation Potentials 8.1 INTRAVALLEY DEFORMATION POTENTIAL: G POINT 8.1.1 Group-IV Semiconductor Alloy A review of the various DPs is given in Adachi [1]. The G-valley DPs (aGc ¼ E1G and Di) in the CB of some non-alloyed ANB8N tetrahedral semiconductors are summarized in Tables 8.1 and 8.2. Tables 8.3 and 8.4 also summarize the G-point DPs a, b, d and Ci in the VB for some cubic and wurtzite semiconductors, respectively. Table 8.1 Intravalley deformation potential, aGc ¼ E1G , for electrons at the G point of some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

aGc (eV)

System

Material

aGc (eV)

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

30.7a,b 15.3a,b 8.24a,b 13.7a,b 7.50b

II–VI

ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb)

4.09b 4.17b 5.83b 27.1b 11.0b 3.96b

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb) InSb (zb)

36.5b 13.3b 11.7b 5.54b 5.64b 6.97b 21.3b 7.14b 11.0 9 11.4 10.2 15

HgTe (zb)

4.60b

a b

G20 -conduction band Calculated

No experimental determinations of the intravalley DPs in the G valley for group-IV semiconductor alloys appear to be available. The interpolated DPs for SixGe1x obtained by Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

260

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 8.2 Intravalley deformation potentials, D1 and D2, for electrons at the G point of some wurtzite III–V semiconductors System

Material

D1 (eV)

D2 (eV)

III–V

AlN GaN

10.23a 9.47a

9.65a 7.17a

a

Calculated

Table 8.3 Deformation potentials, a, b and d, for holes at the G point of some cubic group-IV, III–Vand II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

a (eV)

b (eV)

d (eV)

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

36.1a 5 5.2 3.3a 4.30a

11.1a 2.3 2.4 2.3 2.20a

5.3 4.8 4.1 6.26a

III–V

BN (zb) BP (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb) InSb (zb)

7.3a 4.2a

3.41a 4.9a 4.5a 1.7a 1.5a 2.3a 1.35 2.09a 1.7 1.85 2.4 1.7 1.8 2.0

II–VI

a

Calculated

MgSe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

5.9a 3.15a 2.6a 1.38a 13.33a 1.70a 0.85 0.79a 0.6 1.00a 0.36a 1.0a 2.31a 1.65a 0.79a 0.92a 8.9a 0.55a 0.13a

1.27a 1.1 1.8 1.4 4.7 0.8 1.0 1.24a 1.16a 1.5

3.75a 4.4a 4.3 1.75a 4.4 5.1 5.4 4.3 3.6 5.4 4.4 5.0 4.4 4.4 8.0

DEFORMATION POTENTIALS

261

Table 8.4 Deformation potential Ci for holes at the G point of some wurtzite III–V and II–VI semiconductors (in eV) D1–C1

System

Material

C1

III–V

AlN GaN InN

12.9a 41.4

II–VI

ZnO CdS CdSe

a

3.1 4.05a

C2 8.4a 33.3

3.90 1.36 0.76

D2–C2

C3

C4

C5

C6

11.2 6.67a

4.5a 8.2 4.92a

2.2a 4.1 1.79a

2.6a 4.7

4.1a

4.13 2.28 3.7

1.15 1.54 4.0

1.22 2.34 2.2

1.53 1.20 1.2

2.88 3.0

Calculated

introducing the Si and Ge values in Tables 8.1 and 8.3 into Equation (A.16) are therefore plotted in Figure 8.1. The solid circles in Figure 8.1(b) show the theoretical b values obtained by Schmid et al. [2]. Rieger and Vogl [3] also reported the theoretical b versus x data for SixGe1x, which vary from 2.1 (x ¼ 0) to 2.3 eV (x ¼ 1.0). 0

0 (a)

(b) -1

SixGe1-x a, b, d (eV)

acΓ (eV)

-4 -8 -12

-2 b

-3 -4

-16 -20

d

-5 0

0.2 0.4 0.6 0.8 1.0 x

-6

0

a

0.2 0.4 0.6 0.8 1.0 x

Figure 8.1 (a) CB DP aGc and (b) VB DPs a, b and d for SixGe1x. The solid lines are obtained by introducing the endpoint elemental data into Equation (A.16). The solid circles in (b) show the theoretical b values calculated by Schmid et al. [2]

The E0-gap DP aG0 for some non-alloyed group-IV, III–V and II–VI semiconductors is listed in Table 8.5. Schmid et al. [2] reported a theoretical aG0 value of 11.5 eV for Si0.5Ge0.5. No experimental data are available for group-IV semiconductor alloys.

8.1.2 III–V Semiconductor Ternary Alloy (a) AlGaN The E0-gap DP aG0 can be simply obtained if the pressure coefficient dE0/dp and bulk modulus Bu are available [1]. The pressure coefficient for w-AlxGa1xN has been measured by

262

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 8.5 Hydrostatic deformation potential aG0 for the E0 gap of some cubic and hexagonal semiconductors. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite System

Material

aG0 (eV)

System

Material

aG0 (eV)

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

27a,b 11.84a,b 9.8a 7.04a,b 11.5b

II–VI

MgSe (zb) ZnO (w) ZnS (zb) ZnS (w)

4.2b 3.51 (A) 3.59 (B) 3.81 (C) 5.2 4.7b

BP (zb) AlN (zb) AlN (w) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

17.5b 9.5b 10.3b 9.52b 8.93b 5.9 9.0b 8.8 9.3 8.8 8.3 4.2b 6.0 6.3 7.0

ZnSe (zb) ZnTe (zb) CdS (zb) CdS (w) CdSe (zb) CdSe (w) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

5.1 5.3 0.43b 2.9 0.80b 2.3 2.9 2.16b 2.15b 3.69

III–V

a v b

G250 –Gc20 gap Calculated or estimated

Shan et al. [4]. The x-dependent Bu value for this alloy can be easily obtained by introducing the AlN and GaN values in Table 3.22 of Adachi [1] into the linear interpolation expression. The results obtained are shown in Figure 8.2(a). (b) GaInN The pressure coefficient dE0/dp for w-GaxIn1xN has been measured by Li et al. [5] and also discussed both theoretically and experimentally by Franssen et al. [6]. Figure 8.2(b) shows the aG0 versus x plots for w-GaxIn1xN obtained using the same procedure as in Figure 8.2(a). (c) AlInP Figure 8.3(a) shows the shear DPs b and d versus x for AlxIn1xP. Ishitani et al. [7] determined the shear DP b ¼ 1.67 0.26 eV for AlxIn1xP (0.43 x 0.62) grown on GaAs(100) by MOCVD using PR. This value is plotted in Figure 8.3(a) by the solid circle. The linear interpolation scheme is found to give satisfactory agreement with the experimental data.

DEFORMATION POTENTIALS 0

263

0 (a) w-AlxGa1-xN -4 a0Γ (eV)

a0Γ (eV)

-4

-8

-12

-8

-12 (b) w-GaxIn1-xN

-16

0

0.2 0.4 0.6 0.8 1.0 x

-16

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.2 aG0 for (a) w-AlxGa1xN and (b) w-GaxIn1xN. The solid circles are deduced from the experimental dE0/dp data of (a) Shan et al. [4] and (b) Li et al. [5]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

(d) GaInP The shear DPs b and d versus x for GaxIn1xP are shown plot in Figure 8.3(b). The solid circle represents the experimental data d ¼ 4.0 0.2 eV taken from Bolkhovityanov et al. [8]. This data deviates slightly from the linear interpolation result. 0

0 (a) AlxIn1-xP

-0.8

b

b, d (eV)

-1.6

(b) GaxIn1-xP

-0.8

-2.4

-2.4

-3.2

-3.2

-4.0

b

-1.6

-4.0

d

d

-4.8

0

0.2 0.4 0.6 0.8 1.0 x

-4.8

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.3 Shear DPs b and d for (a) AlxIn1xP and (b) GaxIn1xP. The experimental data in (a) are taken from Ishitani et al. [7] and in (b) from Bolkhovityanov et al. [8]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

(e) AlGaAs Figure 8.4(a) shows the DPs a, b and d for AlxGa1xAs. The experimental data are taken from Qiang et al. [9,10]. The solid lines (a and b) show the linear interpolation results obtained by introducing the GaAs (x ¼ 0) and AlAs (x ¼ 1.0) values in Table 8.3 into Equation (A.4).

264

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 8.4(b) shows the E0-gap DP aG0 for AlxGa1xAs. The solid circles are obtained from the experimental data for dE0/dp (Figure 6.21(b)) using the same procedure as in Figure 8.2(a). The aG0 value is found to be 8.9 eV, i.e. independent of x. 0

0

-1

a

-3

-2

AlxGa1-xAs

b

-3

a0Γ (eV)

a, b, d (eV)

(b)

(a)

-6

-4 -5

-9

d

-6 -7

0

0.2 0.4 0.6 0.8 1.0 x

-12

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.4 (a) DPs a, b and d and (b) aG0 for AlxGa1xAs. The experimental data in (a) are taken from Qiang et al. [9,10]. The aG0 values in (b) are deduced from the experimental dE0/dp data in Figure 6.21(b). The solid lines for a and b in (a) are obtained by introducing the endpoint binary data into Equation (A.4)

(f) AlInAs The DPs a, b and d for AlxIn1xAs are shown in Figure 8.5(a). The experimental data are taken from Yeh et al. [11] (open circle) and Pavesi et al. [12] (solid circle). The E0-gap DP values aG0 measured by Pavesi et al. [12] (solid circle) and Ferguson et al. [13] (solid triangle) are also shown in Figure 8.5(b), together with the endpoint binary data (open squares).

2.0

0

(a)

1.0

AlxIn1-xAs

-4 a

-1.0 -2.0

b

-3.0

a0Γ (eV)

0 a, b, d (eV)

(b)

-2

-6 -8

-10 d

-4.0

0

0.2 0.4 0.6 0.8 1.0 x

-12

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.5 (a) DPs a, b and d and (b) aG0 for AlxIn1xAs. The solid lines in (a) and (b) are obtained by introducing the endpoint binary data into Equation (A.4). The open circle in (a) represents the experimental data of Yeh et al. [11], while the solid circles in (a) and (b) are taken from Pavesi et al. [12]. The solid triangle in (b) also shows the experimental data of Ferguson et al. [13]

DEFORMATION POTENTIALS

265

(g) GaInAs Figure 8.6 shows the E0-gap DP aG0 versus x for GaxIn1xAs. The experimental data obtained by People et al. [14] for x ¼ 0.47 is shown in Figure 8.5(b) by the solid circle, together with the endpoint binary data (open squares). These data give the following quadratic least-squares fit (in eV) aG0 ðxÞ ¼ 6:33:8x þ 1:3x2 ð8:1Þ Wilkinson et al. [15] reported the x-dependent aG0 value for GaxIn1xAs to be aG0 ¼ 7.993.76x eV. However, the InAs value, aG0 ¼ 7.99 eV, obtained from this expression predicts a considerably large pressure coefficient dE0/dp 1.4 101 eV/GPa. A pressure coefficient as large as this has never been reported in the literature. (Only values in the range of dE0/dp ¼ (9.56–11.4) 102 eV/GPa have been reported in the literature [16]). 0

a0Γ (eV)

-2

GaxIn1-xAs

-4 -6 -8 -10 -12

0

0.2

0.4

x

0.6

0.8

1.0

Figure 8.6 aG0 for GaxIn1xAs. The solid circle shows the experimental data of People et al. [14]. The solid line represents the calculated result using Equation (8.1)

(h) GaNAs The shear DP b for dilute-nitride GaNxAs1x has been determined using ER [17] and PR [18]. The data obtained by Zhang et al. [17] (solid circles) and Ya et al. [18] (open circles) are shown in Figure 8.7. These data show a surprising bowing in a small range of alloy compositions and exhibit a minimum at x 1.7 at%. The quadratic least-squares fit of these data can be written as 0 GaNx As1-x

b (eV)

-1 -2 -3 -4

0

1

2

3 x (at%)

4

5

Figure 8.7 Shear DP b for dilute-nitride GaNxAs1x. The experimental data are obtained from Zhang et al. [17] (solid circles) and Ya et al. [18] (open circles). The solid line shows the calculated result using Equation (8.2)

266

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b in eV, x in at%) bðxÞ ¼ 1:850:99x þ 0:29x2

ð8:2Þ

The results contradict the currently held view that the CB is greatly altered but the VB is only weakly perturbed by dilute N doping of III–V semiconductors. (i) GaPAs

a, b, d (eV)

The DPs a, b and d for GaPxAs1x are shown in Figure 8.8. The solid circles represent the experimental b values obtained by Gonzalez et al. [19]. It can be seen that the linear interpolation scheme traces the experimental DP data very well. 2 1 0 -1 -2 -3 -4 -5 -6

a

b

GaPxAs1-x

0

0.2

d

0.4

0.6

0.8

1.0

x

Figure 8.8 DPs a, b and d for GaPxAs1x. The solid circles show the experimental data reported by Gonzalez et al. [19]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

8.1.3 III–V Semiconductor Quaternary Alloy There has been no detailed experimental data relating to a, b or d for any III–V quaternary. Therefore, the linearly interpolated a, b and d values for GaxIn1xPyAs1y/InP using Equation (A.6) are plotted in Figure 8.9(a). The DPs a and d show upward bowing against y, while b varies almost linearly with y. Figure 8.9(b) shows the E0-gap DP aG0 versus y for GaxIn1xPyAs1y/InP. The solid circles represent the experimental data obtained from the pressure coefficients dE0/dp (Figure 6.46(b)) using the same procedure as in Figure 8.2(a). The solid line represents the linearly interpolated aG0 values obtained by introducing the binary data into Equation (A.6). The experimental aG0 values for GaxIn1xPyAs1y/InP are found to be well interpreted by the linear interpolation expression (in eV) aG0 ðxÞ ¼ 7:6 þ 1:6x ð8:3Þ

8.1.4 II–VI Semiconductor Alloy The shear DPs b and d versus x for ZnxCd1xTe are shown in Figure 8.10. The solid circle shows the experimental value b ¼ 1.07 0.06 eV for x ¼ 0.605 determined by Pelhos et al. [20].

DEFORMATION POTENTIALS 1

-3

0

Gax In1-x Py As1-y /InP

a

-6

b

-2

a0Γ (eV)

a, b, d (eV)

-1

-3

-9

d

-4 -5 -6 0

267

(a)

(b)

-12 0

0.2 0.4 0.6 0.8 1.0 y

0.2 0.4 0.6 0.8 1.0 y

Figure 8.9 (a) DPs a, b and d and (b) aG0 for GaxIn1xPyAs1y/InP. The solid circles in (b) are deduced from the experimental dE0/dp data in Figure 6.46(b). The solid lines in (a) and (b) are obtained by introducing the binary data into Equation (A.6) 0

b, d (eV)

-1

b

-2 ZnxCd1-xTe

-3 -4

d

-5 -6

0

0.2

0.4

0.6

0.8

1.0

x

Figure 8.10 Shear DPs b and d for ZnxCd1xTe. The solid circle shows the experimental data reported by Pelhos et al. [20]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

The pressure coefficient dE0/dp has been measured on some II–VI semiconductor alloys, such as w-MgxZn1xO [21], w-ZnxCd1xS [22], c-ZnOxSe1x [23], ZnSxSe1x [24], ZnSxTe1x [25] and ZnSexTe1x [26]. By introducing these pressure coefficients and interpolated Bu values (Tables 3.17 and 3.22 in Adachi [1]) into Equation (8.14) of Adachi [1], aG0 for such II–VI semiconductor alloys can be obtained.

8.2 INTRAVALLEY DEFORMATION POTENTIAL: HIGH-SYMMETRY POINTS 8.2.1 Group-IV Semiconductor Alloy The L-valley DPs for some non-alloyed ANB8N tetrahedral semiconductors are summarized in Tables 8.6–8.8. Table 8.9 also summarizes the X (D)-valley DPs for some non-alloyed groupIV and III–V semiconductors.

268

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 8.6 Hydrostatic E1 and shear deformation potentials E2 for electrons at the L point of some cubic group-IV and III–V semiconductors System

Material

IV

Si Ge

a b

E1 (eV)

E2 (eV)

3.1a 3.8

18.0a 15.9

System

Material

III–V

c-BN c-AlN AlAs b-GaN GaAs GaSb

E1 (eV)

E2 (eV) 27.9a 25.5a

4.2b

27.5a 14.5 17.5

2 3.2

Calculated Estimated

Table 8.7 Deformation potentials, D53 and D33 , for holes at the L point of some cubic group-IV, III–V and II–VI semiconductors determined experimentally System

Material

IV

Si Ge

III–V

GaAs InP

D53 (eV) 4.3 3.7 6.4 12.9

D33 (eV)

System

Material

D53 (eV)

D33 (eV)

4.6 5.6 (E1) 6.2 (E1 þ D1)

II–VI

ZnSe ZnTe

27 15

17 29

5.4 4.1

pﬃﬃﬃ Table 8.8 Hydrostatic D11 ¼ 3aL1 and interband deformation potentials D51 for the E1 and E1 þ D1 gaps of some cubic group-IV, III–V and II–VI semiconductors determined experimentally System

Material

IV

Si Ge

III–V

GaAs GaSb InP InSb

II–VI

ZnSe ZnTe

D11 (eV) 9.0 8.7 8.3 12.3 (E1) 17.7 (E1 þ D1) 9.2 7.4 (E1) 8.5 (E1 þ D1) 5.8 5.5

D51 (eV) 9 12.2 12.0 7.4 (E1) 20.4 7.4 (E1) 6.5 (E1 þ D1) 30 40

DEFORMATION POTENTIALS

269

Table 8.9 Hydrostatic E1 and shear deformation potentials E2 for electrons at the X point of some cubic group-IV and III–V semiconductors System

Material

IV

Si Ge

a b

E1 (eV)

E2 (eV)

4.2 5.75a

9.6 9.75a

System

Material

III–V

c-BN c-AlN AlP AlAs AlSb b-GaN GaP GaAs GaSb InP InAs InSb

E1 (eV) 5.5 1.81a 1.20 a

6.8a 2.7 1.05b 1.99a 1.85a 1.59a 1.56a

E2 (eV) 17.9a 6.6a 6.75a 6.9 5.4 7.1a 6.3 6.5 6.46a 3.3a 3.7a 4.53a

Calculated Estimated

Although there have been several theoretical studies on the DPs at the high-symmetry points of SixGe1x [2,3], no experimental determinations appear to be available for any group-IV semiconductor alloy. Figure 8.11 shows the linearly interpolated L- and X-valley DPs E1(L) and E1(X) at the CB, respectively, obtained by introducing the Si and Ge values in Tables 8.6 and 8.9 into Equation (A.16). The crossing of the lowest-lying CB states from the L point to the X (D) point can be seen at x 0.15 (Figure 6.8). Thus, the nature of the conduction electron in SixGe1x changes from ‘Ge-like’ to ‘Si-like’ at x 0.15. 8 L-X (Δ) crossing

E1(L) (eV)

-1.6

SixGe1-x

6

-2.4 4 -3.2 2

-4.0 -4.8

E1(X) (eV)

-0.8

(Ge-like)

0

0.2

0.4

x

0.6

0.8

0 1.0

Figure 8.11 L- and X-valley DPs E1(L) and E1(X) at the CB for SixGe1x. The solid lines are obtained by introducing the endpoint elemental data into Equation (A.16). The dashed line indicates the L–X (D) crossing composition xc 0.15

8.2.2 III–V Semiconductor Alloy Figure 8.12 shows the X-valley DP E1 in the CB versus x for AlxGa1xAs. The experimental data are taken from Adachi [27]. These data provide the following x variation: E1 ¼ 1.05 þ 0.15x eV. The solid line in Figure 8.12 shows the result of this variation.

270

PROPERTIES OF SEMICONDUCTOR ALLOYS

E1(X) (eV)

2.0 AlxGa1-x As

1.5 1.0 0.5 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 8.12 X-valley DP E1 in the CB for AlxGa1xAs. The experimental data are taken from Adachi [27]. The solid line shows the linearly interpolated result using the endpoint binary data

Figure 8.13 plots the L-valley DP D33 in the VB for GaPxAs1x. The solid circles show the experimental data obtained by Gonzalez et al. [19] determined using ER. The solid line represents the calculated result of D33 ¼ 5.4 þ 5.0x eV. This expression predicts a GaP (x ¼ 1.0) value of 0.4 eV. The experimental D53 and D33 values reported for non-alloyed ANB8N tetrahedral semiconductors are limited to Si, Ge, GaAs, InP, ZnSe and ZnTe (Table 8.7, see also Adachi [16,28,29]). 0

D33 (eV)

-1 GaPx As1-x

-2 -3 -4 -5 -6 0

0.2

0.4

x

0.6

0.8

1.0

Figure 8.13 L-valley DP D33 in the VB for GaPxAs1x. The solid circles show the experimental data of Gonzalez et al. [19]. The solid line represents the calculated result of D33 ¼ 5.4 þ 5.0x eV

8.2.3 II–VI Semiconductor Alloy No detailed data are available for II–VI semiconductor alloys.

8.3 INTERVALLEY DEFORMATION POTENTIAL 8.3.1 Group-IV Semiconductor Alloy The intervalley DPs for some non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Tables 8.10 and 8.11. Unfortunately, no detailed data are available for group-IV semiconductor alloys.

DEFORMATION POTENTIALS

271

Table 8.10 Intervalley deformation potential Dij for electrons in some cubic group-IV, III–V and II–VI semiconductors (in eV/A) System

Material

IV

Diamond Si Ge

2.0

III–V

AlP AlAs AlSb GaP GaAs GaSb InP InAs InSb

5.0 1.6–2.3 2.3–3.4 0.7–1.1 1.5–9.5 2.7–2.8 1.3–2.7 1.0–2.0 1.1–4.3

5.0 3.1 1.3–4.9 0.8–1.1 5.2–15 2.5–4.5 1.6 2.0–2.2 3.3–4.9

II–VI

b-ZnS ZnSe ZnTe CdTe

2.18–4.13 2.17–2.71 3.19–3.31 1.68–1.76

1.10–1.89 0.72–1.37 1.17–1.43 0.40–1.23

a

DGL

DGXa

DLL

10.0

2.63 0.2–3.0

DXX 8.0 0.15–4.0 0.79–9.5

0.3–1.0 1.6 0.5–0.6 0.6 5 0.6–1.2 0.3–0.9 1.1 0.3–0.6

8.1 4.7 9.5 3.0 10 6.0 3.6 2.5 6.8

DLX 4.0 4.1 0.4–1.7 0.8–3.7 0.4–1.6 2.75–3.1 1.0–2.2 0.7–3.3 0.6–1.9 0.2–2.9

DGX(1) and DGX(3)

Table 8.11 Intervalley deformation potential Dij for electrons in some hexagonal III–V semiconductors

Dij (eV/A)

Material

w-AlN a-GaN InN

Equivalent valley

Nonequivalent valley

10 5–10 10

10 10 10

8.3.2 III–V Semiconductor Alloy Parker et al. [30] observed field-assisted emission from a heterostructure with a GaAs–Al0.25 Ga0.75As emitter layer and derived information on hot-electron energy distributions at the low electron density limit. From computer-modeled analysis, they deduced the intervalley coupling constants Dij for Al0.25Ga0.75As. These results are shown in Figure 8.14 together with those for AlAs and GaAs (Table 8.10).

272

PROPERTIES OF SEMICONDUCTOR ALLOYS 15

15 AlxGa1-x As

Dij (eV/Å)

10

10

DΓL

5

5

0 15

0 15

10

10

DΓX

5

5

0 15

0

10

DXX

DLX

0

0.2

0.4

x

0.6

0.8

1.0

DLL

5 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 8.14 Intervalley coupling constants Dij for AlxGa1xAs. The solid circles show the Al0.25Ga0.75As values deduced from field-assisted emission data reported by Parker et al. [30]

8.3.3 II–VI Semiconductor Alloy No detailed data are available for II–VI semiconductor alloys.

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] U. Schmid, N.E. Christensen, and M. Cardona, Solid State Commun. 75, 39 (1990). [3] M.M. Rieger and P. Vogl, Phys. Rev. B 48, 14276 (1993). [4] W. Shan, J.W. Ager III, K.M. Yu, W. Walukiewicz, E.E. Haller, M.C. Martin, W.R. McKinney, and W. Yang, J. Appl. Phys. 85, 8505 (1999). [5] S.X. Li, J. Wu, W. Walukiewicz, W. Shan, E.E. Haller, H. Lu, W.J. Schaff, Y. Saito, and Y. Nanishi, Phys. Status Solidi B 241, 3107 (2004). [6] G. Franssen, I. Gorczyca, T. Suski, A. Kami nska, J. Pereiro, E. Mu~ noz, E. Iliopoulos, A. Georgakilas, S.B. Che, Y. Ishitani, A. Yoshikawa, N.E. Christensen, and A. Svane, J. Appl. Phys. 103, 033514 (2008). [7] Y. Ishitani, H. Hamada, S. Minagawa, H. Yaguchi, and Y. Shiraki, Jpn. J. Appl. Phys. 36, 6607 (1997). [8] Y.B. Bolkhovityanov, A.S. Jaroshevich, M.A. Revenko, H.E. Scheibler, and A.S. Terekhov, Semicond. Sc. Technol. 11, 1847 (1996). [9] H. Qiang, F.H. Pollak, and G. Hickman, Solid State Commun. 76, 1087 (1990). [10] H. Qiang, F.H. Pollak, and R.N. Sacks, Solid State Commun. 84, 51 (1992). [11] C.N. Yeh, L.E. McNeil, R.E. Nahory, and R. Bhat, Phys. Rev. B 52, 14682 (1995). [12] L. Pavesi, R. Houdre, and P. Giannozzi, J. Appl. Phys. 78, 470 (1995). [13] I.T. Ferguson, T.P. Beales, T.S. Cheng, C.M. Sotomayor-Torres, and E.G. Scott, Semicond. Sci. Technol. 4, 243 (1989). [14] R. People, A. Jayaaraman, K.W. Wecht, D.L. Sivco, and A.Y. Cho, Appl. Phys. Lett. 52, 2124 (1988). [15] V.A. Wilkinson, A.D. Prins, J.D. Lambkin, E.P. OReilly, D.J. Dunstan, L.K. Howard, and M.T. Emeny, Phys. Rev. B 42, 3113 (1990).

DEFORMATION POTENTIALS

273

[16] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [17] Y. Zhang, A. Mascarenhas, H.P. Xin, and C.W. Tu, Phys. Rev. B 61, 4433 (2000). [18] M.H. Ya, Y.F. Chen, and Y.S. Huang, J. Appl. Phys. 92, 1446 (2002). [19] Y. Gonzalez, G. Armelles, and L. Gonzalez, J. Appl. Phys. 76, 1951 (1994). [20] K. Pelhos, S.A. Lee, Y. Rajakarunanayake, and J.L. Reno, Phys. Rev. B 51, 13256 (1995). [21] J.A. Sans and A. Segura, High Pressure Res. 24, 119 (2004). [22] A. Beliveau and C. Carlone, Phys. Rev. B 41, 9860 (1990). [23] W. Shan, W. Walukiewicz, J.W. Ager III, K.M. Yu, J. Wu, E.E. Haller, Y. Nabetani, T. Murakawa, Y. Ito, and T. Matsumoto, Appl. Phys. Lett. 83, 299 (2003). [24] E. Griebl, G.F. Sch€otz, C. Birzer, W. Kerner, T. Reisinger, B. Hahn, and W. Gebhardt, Acta Phys. Polon. A 88, 995 (1995). [25] W. Walukiewicz, W. Shan, K.M. Yu, J.W. Ager III, E.E. Haller, I. Miotkowski, M.J. Seong, H. Alawadhi, and A.K. Ramdas, Phys. Rev. Lett. 85, 1552 (2000). [26] J. Wu, W. Walukiewicz, K.M. Yu, W. Shan, J.W. Ager III, E.E. Haller, I. Miotkowski, A.K. Ramdas, and C.-H. Su, Phys. Rev. B 68, 033206 (2003). [27] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [28] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [29] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [30] T.R. Parker, C.C. Phillips, and P.C. May, Phys. Rev. B 51, 4264 (1995).

9 Heterojunction Band Offsets and Schottky Barrier Height 9.1 HETEROJUNCTION BAND OFFSETS 9.1.1 General Considerations One of the most important parameters for the design and analysis of heterojunction and QW electronic and optoelectronic devices is the heterojunction band offset. The band offset is a consequence of the difference between the band-gap energies of two semiconductors. As shown in Figure 9.1, the energy difference is distributed between a CB offset DEc and a VB offset DEv. In a type I (straddling lineup), we obtain DEg ¼ DEc þ DEv

ð9:1Þ

while for type II (broken-gap and staggered lineups) the relationship is given by DEg ¼ jDEc DEv j

ð9:2Þ

where DEg ¼ jEg1 Eg2j is the band-gap energy difference. Since the temperature variations of the band-gap energies are very similar among various semiconductors [1], the band offsets and offset ratio can usually be assumed to be independent of temperature.

9.1.2 Group-IV Semiconductor Heterostructure System (a) CSi/Si The CxSi1x/Si heterostructure shows a biaxial tensile strain in the alloy layer. The biaxial strain or stress in the coherently strained QW layers splits the LH and HH bands so that the LH band is highest in CxSi1x layer. Similarly, for CxSi1x layers with smaller x compositions, the lowest CB is at the X (D) band. Brunner et al. [2] measured near-band-edge emission from pseudomorphic CxSi1x/Si QW structures with x up to 2 at%. They found a linear decrease in the PL emission peak with increasing x, which is about 30% larger than the expected band-gap reduction induced by strain. This might indicate that incorporation of C reduces the intrinsic band-gap energy. The trend for decreasing CxSi1x band-gap energy was also proposed by detailed binding calculations [3]. The band-offset values for CxSi1x/Si heterostructure have been determined experimentally by several authors [4, 5]. Houghton et al. [4] confirmed a type-I alignment in CxSi1x/Si with x ¼ 0.5 1.7 at% and also observed an elastic-strain-induced transition from type I to type II in Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

276

PROPERTIES OF SEMICONDUCTOR ALLOYS (a)

(b)

(c)

ΔEc ΔEc

Eg1

ΔEv

Eg2 ΔEv

Figure 9.1 Schematic energy-band diagrams showing three representative types of heterostructure interfaces: (a) type I (straddling lineup), (b) type II-misaligned (broken-gap lineup) and (c) type IIstaggered (staggered lineup)

CxSi1x/Si QWs. The band-offset ratio obtained by these authors is DEc : DEv ¼ 65 : 35 with Eg(Si) Eg(CxSi1x). Williams et al. [5] also obtained a band-offset ratio of about 70 : 30 (a)

(b) ΔEc=0.3ΔEg ΔEc=0.7ΔEg

ΔEv=1.3ΔEg

ΔEv=0.3ΔEg Si

Cx Si1-x

Si

Six Ge1-x

Figure 9.2 Schematic energy-band alignments for (a) CxSi1x/Si and (b) SixGe1x/Si heterostructures obtained by Williams et al. [5] and Cheng et al. [12], respectively

for x ¼ 0.5 1.7 at%. The corresponding band lineup is shown schematically in Figure 9.2(a). An ab initio calculation confirms the offset ratio of 70 : 30 [6]. (b) SiGe/Si Previous studies on the band alignment of the SixGe1x/Si heterostructure suggest type-I [7, 8] or type-II behavior [9–12]. By employing a wafer bending technique, Thewalt et al. [11] observed both type-I and type-II behaviors respectively, in PL of an UHV-CVD-grown Si0.7Ge0.3/Si(100) QW at high and low laser powers. They concluded that a determination of type-I alignment [7, 8] is a result of the band-bending effects due to high excitation. More recently, Cheng et al. [12] made PL measurements on UHV-CVD-grown and MBE-grown SixGe1x/Si MQWs and concluded that the band alignment was type II with DEc ¼ 0.3DEg and DEv ¼ 1.3DEg, as shown in Figure 9.2(b). (c) CSiGe/Si The incorporation of C into SixGe1x can compensate for some of the biaxial compressive strain in the SixGe1x/Si heterostructure. The incorporation of C evidently lowers the CB and VB energies and decreases the intrinsic band gap in SixGe1x. The intrinsic band alignment of SixGe1x/Si is always type-II in character. Neglecting the effect of strain, therefore, we can

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

277

expect a transition from type II to type I by incorporating C into SixGe1x. In fact, Stein et al. [13, 14] and Hartmann et al. [15] concluded that the band alignment in the CxSiyGe1xy/Si heterostructure is type I, regardless of whether the strain is compensated or not. However, a staggered type-II alignment has been reported in strain-relaxed Ge-rich CxSiyGe1xy/Si heterostructures (x ¼ 0.01 0.02 and y ¼ 0.10 0.13), with electrons (holes) localized in the Si (CxSiyGe1xy) layer [16]. The band offsets DEc and DEv determined were typically 0.4 and 0.6 eV, respectively. (d) CSi/SiGe Using a wafer bonding technique, Houghton et al. [4] obtained a type-II transition in a C0.01Si0.99/Si0.84Ge0.16/Si heterostructure, with electrons (holes) localized in the C0.01Si0.99 (Si0.84Ge0.16) layer.

9.1.3 III–V Semiconductor Heterostructure System: Lattice-matched Ternary-alloy System (a) GaInP/GaAs The band-offset ratio DEc : DEv determined experimentally for the Ga0.52In0.48P/GaAs heterostructure ranges widely from 13 : 87 to 63 : 37 [17]. The mean offset ratio gives DEc : DEv ¼ 33 : 67. The corresponding band offsets are DEc 0.16 eV and DEv 0.33 eV. The existence of spontaneous ordering in the Ga0.52In0.48P layer could significantly alter the band offset [17]. Thus, it appears that the ordering effect itself might have contributed to the larger scatter in the reported values, at least to some extent. The ordering effect can also change the band alignment from type I to type II, as schematically shown in Figure 9.3. (a)

(b)

(c)

ΔEc =0.16 eV GaAs

1.43 eV

ΔEc =0.33 eV

Fully disordered Ga 0.52In 0.48P

Partly ordered Fully ordered Ga 0.52In 0.48P Ga 0.52In 0.48P

Figure 9.3 Schematic energy-band diagram showing the effect of spontaneous ordering for Ga0.52In0.48P/GaAs heterostructure

Zhang et al. [17] obtained theoretically a transition from type I to type II at h ¼ 0.46 (0.54) in the GaxIn1xP/GaAs heterostructure with x ¼ 0.50 (0.52), where h is the so-called order parameter. (b) GaInP/AlInP Patel et al. [18] obtained the band-offset ratio DEc : DEv ¼ 52 : 48 in the Ga0.52In0.48P/ Al0.5In0.5P heterostructure, where the CB minimum is in the X valley for Al0.5In0.5P and in

278

PROPERTIES OF SEMICONDUCTOR ALLOYS

the G valley for Ga0.52In0.48P (i.e. DEc ¼ EcX(Al0.5In0.5P) EcG(Ga0.52In0.48P)). More recently, Dawson et al. [19] revised the offset ratio to DEc : DEv ¼ 67 : 33 from low-temperature PL measurements. (c) GaInP/AlGaAs The band alignment in the Ga0.52In0.48P/AlxGa1xAs heterostructure is expected to change from a straddling to a staggered type as the Al content x increases from x ¼ 0 (GaAs), as shown in Figure 9.4. Kim et al. [20] reported a transition occurring at about x ¼ 0.12 (Figure 9.4(b)). (a)

(b)

(c)

ΔEc =0.16 eV

Ga 0.52In 0.48P GaAs (x=0)

x=0.12

x> 0.12

ΔEv =0.33 eV Ga 0.52In 0.48P/Al xGa 1-xAs

x

Figure 9.4 Schematic energy-band diagram for Ga0.52In0.48P/GaxAl1xAs heterostructure with (a) x ¼ 0, (b) x ¼ 0.12 and (c) x > 0.12

(d) AlGaAs/GaAs The pioneering work of Dingle et al. [21, 22] on the AlxGa1xAs/GaAs MQW structure gave the offset ratio of DEc : DEv ¼ 85 : 15. Although this ratio had long been accepted, some studies required different ratios in the range of (0.62 0.66) : (0.38 0.34) to explain electrical and photoelectric data. The discrepancy with Dingles result was attributed to compositional grading or any interface states at the AlxGa1xAs/GaAs heterojunction. However, in 1984 Miller et al. [23, 24] reported values of 51 : 49 and 57 : 43 using PL from parabolic and rectangular QWs. Subsequently, Dugan et al. [25] arrived at 65 : 35. By averaging the recently published data, we recommend an offset ratio of DEcG : DEv ¼ 63 : 37. Using this ratio and the E0 and EgX values shown in Table 6.11, we obtain the DEc and DEv versus x plots for the AlxGa1xAs/GaAs heterostructure. Figure 9.5 shows these results. We can see that the band lineup is type I over the whole composition range 0 x 1.0 [26]. Note, however, that the CB minimum changes from the G point ðDEcG Þ to the X point ðDEcX Þ at x 0.43. The band offsets can be finally approximated for x 0.8 as (in eV) DEcG ðxÞ ¼ 0:85x

ð9:3aÞ

DEcX ðxÞ ¼ 0:480:30x

ð9:3bÞ

DEv ðxÞ ¼ 0:50x

ð9:3cÞ

ΔEc (eV)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT 1.2 1.0 0.8 0.6 0.4 0.2 0

279

AlxGa1-xAs/GaAs

ΔEcX

ΔEcΓ

ΔEv (eV)

Eg(GaAs)=1.43 eV

0 -0.2 -0.4 -0.6 -0.8 0

ΔEv

0.2

0.4

x

0.6

0.8

1.0

Figure 9.5 A full AlxGa1xAs/GaAs heterostructure band diagram obtained by assuming a band-offset ratio of DEcG : DEv ¼ 63 : 37 and using E0 and EgX in Table 6.11 (solid lines). The dashed lines represent the linear variations of DEc and DEv given by Equation (9.3)

(e) AlInAs/InP The Al0.48In0.52As/InP interface is the least well characterized [27]. The staggered type-II alignment with holes localized in the Al0.48In0.52As layer is generally agreed upon. A CB offset of DEc ¼ 2.86DEg has been reported by B€ ohrer et al. [28]. The direct and inverse heterointerface properties have been studied for the Al0.48 In0.52As/InP heterostructure (Al0.48In0.52As layer grown on InP versus InP layer grown on Al0.48In0.52As) [29, 30]. The clear noncommutativity of 100 20 meV [29] and 53 10 meV [30] has been observed for DEc. (f) GaInAs/InP The band offsets in the Ga0.47In0.53As/InP heterostructure have been studied both theoretically and experimentally [27]. We obtain an averaged experimental offset ratio of DEc : DEv ¼ 38 : 62. The corresponding band alignment is shown in Figure 9.6(a). (b)

(a) ΔEc=0.27 eV

InP

Ga 0.47 In 0.53 As

ΔEv=0.45 eV

ΔEc=0.51 eV

Al 0.48 In 0.52 As

ΔEv=0.22 eV

Figure 9.6 Schematic energy-band alignments for (a) Ga0.47In0.53As/InP and (b) Ga0.47In0.53As/ Al0.48In0.52As heterostructures. The band offsets DEc and DEv are obtained by averaging the literature data

280

PROPERTIES OF SEMICONDUCTOR ALLOYS

The direct and inverse heterointerface properties have been studied on the Ga0.47In0.53As/ InP heterointerface [30, 31]. Substantially large noncommutativity has been reported. The cause of the noncomutativity is attributed to a difference in the chemical nature of the direct and inverse interfaces [31]. A significant nontransitivity for the average band offsets has also been found in the InPAlxIn1xAsGaxIn1xAs family [29, 30]. (g) GaInAs/AlInAs Like Ga0.47In0.53As, Al0.48In0.52As can be grown lattice-matched to InP. The band-gap difference DEg between these ternaries is about 0.73 eV. The band offsets in the Ga0.47 In0.53As/Al0.48In0.52As heterostructure have been determined by several authors [27, 32–34]. Averaging these results produces the offset ratio of DEc : DEv ¼ 70 : 30. The corresponding band lineup is shown in Figure 9.6(b). (h) InAsSb/GaSb InAs0.91Sb0.09 can be grown lattice-matched to GaSb. A broken type of band lineup is accepted for the InAs0.91Sb0.09/GaSb heterostructure [35–37]. Mebarki et al. [36] reported band offsets of DEc ¼ 0.82 eV and DEv ¼ 0.36 eV, respectively. The band lineup for this heterojunction system is illustrated in Figure 9.7.

GaSb

ΔEv =0.36 eV

ΔEc =0.82 eV

InAs0.91Sb0.09

Figure 9.7 Schematic energy-band diagram for InAs0.91Sb0.09/GaSb heterostructure obtained by Mebarki et al. [36]

9.1.4 III–V Semiconductor Heterostructure System: Lattice-matched Quaternary Alloy (a) GaInPAs/InP Although the straddling alignment is generally agreed upon, there is considerable disagreement regarding the band offsets of the GaxIn1xPyAs1y/InP heterostructure [27]. Let us assume a band-offset ratio of DEc : DEv ¼ 38 : 62, which is derived from the Ga0.47In0.53As/InP heterostructure. Using this ratio and E0 in Table 6.28, we obtain the y-dependent DEc and DEv values for the GaxIn1xPyAs1y/InP and GaxIn1xPyAs1y/Ga0.47In0.53As heterostructures. The results can be approximated as (in eV) DEc ðyÞ ¼ 0:230:23y

ð9:4aÞ

DEv ðyÞ ¼ 0:370:37y

ð9:4bÞ

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

281

for the GaxIn1xPyAs1y/InP heterostructure and DEc ðyÞ ¼ 0:23y

ð9:5aÞ

DEv ðyÞ ¼ 0:37y

ð9:5bÞ

for the GaxIn1xPyAs1y/Ga0.47In0.53As heterostructure. (b) AlGaAsSb/GaSb The band offsets in a perfectly lattice-matched Al0.47Ga0.53As0.04Sb0.96/GaSb heterostructure were determined to be DEc ¼ 0.35 eV and DEv ¼ 0.24 eV, respectively, furnishing a fractional ratio of DEc : DEv ¼ 59 : 41 [38]. (c) AlGaAsSb/InP Ostinelli et al. [39] carried out PL on an Al0.168Ga0.832AsSb/InP heterostructure and obtained staggered type-II offsets of DEc ¼ 0.32 eV and DEv ¼ 0.66 eV with electrons (holes) localized in the InP (Al0.168Ga0.832AsSb) layer. These results give DEc ¼ 0.94DEg and DEv ¼ 1.94DEg. (d) AlGaAsSb/InAs Nelson et al. [40] measured PL spectra of the Al0.8Ga0.2As0.14Sb0.86/InAs heterostructure and obtained a staggered lineup with DEc ¼ 1.60 eV and DEv ¼ 0.24 eV with electrons (holes) localized in the InAs (Al0.8Ga0.2As0.14Sb0.86) layer. These results predicted the relationship DEc ¼ 1.18DEg and DEv ¼ 0.18DEg. (e) GaInAsSb/GaSb The band lineup for GaxIn1xAsySb1y/GaSb heterostructure is believed to be type II in nature. Mikhailova and Titkov [41] reviewed the topic. Averaging the experimental data in this review gives DEc ¼ 1.62DEg and DEv ¼ 0.62DEg. These relationships indicate that the transition composition from broken-gap to staggered lineup will be at x 0.24. Afrailov et al. [42] observed a broken-gap character at x ¼ 0.11, whereas Mebarki et al. [43] found the staggered band offsets to be DEc ¼ 0.33 0.05 eV and DEv ¼ 0.12 0.05 eV (x ¼ 0.77) with electrons localized in the GaxIn1xAsySb1y layer. (f) GaInAsSb/InP The band-offset ratio of DEc : DEv ¼ 30 : 70 in the Ga0.64In0.36As0.84Sb0.16/InP heterostructure was obtained by Chang et al. [44] from optical absorption measurements. (g) GaInAsSb/InAs The band lineups in LPE-grown GaxIn1xAsySb1y/InAs heterostructure were investigated by Mikhailova et al. [45]. The broken-gap lineup was observed in the composition range 0.77 x 0.97 and the staggered lineup in the range 0 < x < 0.7.

282

PROPERTIES OF SEMICONDUCTOR ALLOYS

(h) AlGaAsSb/GaInAsSb The band offsets in the Al0.22Ga0.78As0.02Sb0.98/Ga0.75In0.25As0.04Sb0.96 MQW structure grown on GaSb(100) were determined from optical absorption and PL measurements [46]. The offset ratio was determined to be DEc : DEv ¼ 66 : 34. (i) AlInAsSb/GaInAsSb Chang et al. [47] grew Al0.66In0.34As0.85Sb0.15/Ga0.64In0.36As0.84Sb0.16 MQW structures on InP (100) by MOCVD and carried out low-temperature PL measurements. The band-offset ratio estimated from this study was DEc : DEv ¼ 75 : 25. (j) AlGaInP/AlInP The band alignment in (Al0.7Ga0.3)0.53In0.47P/AlxIn1xP heterostructures was investigated by Ishitani et al. [48] using PL spectroscopy. They found that the X-valley discontinuity DEcX decreases with increasing x (0.47 x 0.61). The band-offset ratio obtained was DEc : DEv ¼ 75 : 25 for x ¼ 0.53. (k) AlGaInP/GaInP

ΔEv (eV)

ΔEc (eV)

The band-offset ratios in (AlxGa1x)0.53In0.47P/Ga0.52In0.48P with x in the direct band-gap region (x < 0.65, see Figure 6.49) varied from DEcG : DEv ¼ 49 : 41 to 70 : 30 [49–53]. Averaging these data gives DEcG : DEv ¼ 65 : 35. The corresponding band offsets DEcG , DEcX and DEv are plotted against x in Figure 9.8. The band offsets can now be written as (in eV)

0.6 0.5 0.4 0.3 0.2 0.1 0 0 -0.1 -0.2 -0.3 0

DEcG ¼ 0:43x

ð9:6aÞ

DEcX ¼ 0:360:16x

ð9:6bÞ

DEv ¼ 0:24x

ð9:6cÞ

(AlxGa1-x)0.53In0.47P/Ga0.52In0.48P

ΔEcX

ΔEcΓ Eg~1.9 eV (Ga0.52In0.48P)

ΔE v

0.2

0.4

x

0.6

0.8

1.0

Figure 9.8 A full (AlxGa1x)0.53In0.47P/Ga0.52In0.48P heterostructure band diagram obtained by assuming a band-offset ratio of DEcG : DEv ¼ 65 : 35 and using E0 and EgX in Table 6.28 (solid lines). The dashed lines represent the linear variations of DEc and DEv given by Equation (9.6)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

283

The band offsets in (AlxGa1x)0.53In0.47P/Ga0.52In0.48P with x in the indirect band-gap region were studied by several authors [54, 55]. The effects of long-range ordering on the band alignment are discussed by Shao et al. [56]. (l) AlGaInAs/GaInAs

ΔEv (eV)

ΔEc (eV)

The band offsets in (AlxGa1x)0.48In0.52As/Ga0.47In0.53As were determined from I V [57] and PL and PLE measurements [58]. The offset ratios determined from these studies were DEc : DEv ¼ 72 : 28 and 73 : 27, respectively. Assuming DEc : DEv ¼ 73 : 27 and using E0 in Table 6.28, we can obtain the x-dependent DEc and DEv. The results are shown in Figure 9.9, and can be given by (in eV)

0.6 0.5 0.4 0.3 0.2 0.1 0 0 -0.1 -0.2 -0.3 0

DEc ðxÞ ¼ 0:54x

ð9:7aÞ

DEv ðxÞ ¼ 0:20x

ð9:7bÞ

(AlxGa1-x)0.48In0.52As/Ga0.47In0.53As ΔEc

Eg~0.75 eV (Ga0.47In0.53As) ΔEv

0.2

0.4

x

0.6

0.8

1.0

Figure 9.9 A full (AlxGa1x)0.48In0.52As/Ga0.47In0.53As heterostructure band diagram obtained by assuming a band-offset ratio of DEc : DEv¼73 : 27 and using E0 in Table 6.28

9.1.5 III–V Semiconductor Heterostructure System: Lattice-mismatched Alloy System (a) w-AlGaN/w-GaN The straddling lineup is generally agreed upon, but there is considerable disagreement regarding the band offsets between AlxGa1xN (AlN) and GaN reported by different authors [59–65]. Using the mean value of these data, we obtain DEc : DEv ¼ 65 : 35. Using E0 ¼ 6.2 eV (AlN) and 3.420 eV (GaN) in Table 6.2, we obtain the band offsets for the AlxGa1xN/GaN heterostructure as follows (in eV) DEc ðxÞ ¼ 1:81x

ð9:8aÞ

DEv ðxÞ ¼ 0:97x

ð9:8bÞ

284

PROPERTIES OF SEMICONDUCTOR ALLOYS

Dependence of the AlN/GaN band discontinuity on growth temperature was determined using XPS [66]. A large strain-induced asymmetry of the band offset was suggested from an ab initio electronic structure study [67]. (b) w-AlInN/w-InN The VB offsets DEv ¼ 3.10 0.04 eV [68] and 4.0 0.2 eV [69] were determined in an AlN/ InN heterointerface using photoelectron spectroscopy. These DEv values and values of E0 ¼ 6.2 eV (AlN) and 0.70 eV (InN) in Table 6.2 provide the band-offset ratios DEc : DEv 44 : 56 and 27 : 73, respectively. (c) w-GaInN/w-GaN The band offsets in the GaxIn1xN(InN)/GaN heterostructure were determined using various techniques [70–74]. The mean offset ratio obtained from these studies was DEc : DEv ¼ 67 : 33. (d) GaInAs/GaAs The band discontinuity in a strained-layer system depends not only on the heterostructure system involved but also on the amount of mismatch strain at the interface. The strain field can produce marked effects on the electronic properties through the DP interactions. The hydrostatic component of the strain causes a shift in the bulk energy levels of the strained layer, while the shear component causes splitting of certain degenerate VB levels, namely, the HH and LH levels. The exact energy levels of the heterostructure layer should, therefore, be determined including the strain modification of the layer. In the case of biaxial strain parallel to [010] and [001], the strain components in GaxIn1xAs/ GaAs(100) heterojunctions are exx ¼ eyy ¼ d; ezz ¼

2C12 d; exy ¼ eyz ¼ ezx C11

with d¼

Da a

ð9:9Þ

ð9:10Þ

where d is defined to be positive for compressive strain, Cij is the elastic stiffness constant of GaxIn1xAs and Da is the lattice-constant difference between GaxIn1xAs and GaAs. The corresponding change in the band-gap energy for GaxIn1xAs layer can be written as DEc;v1 ¼ DEc;v2 ¼

2aG0

C11 C12 C11 þ 2C12 1 þb d ¼ dh þ dEs 2 C11 C11

C11 C12 C11 þ 2C12 1 2aG0 b d ¼ dh dEs 2 C11 C11

ð9:11aÞ ð9:11bÞ

where v1 and v2 represent the j3/2, 3/2> (HH-like) and j3/2, 1/2> (LH-like) bands, respectively, aG0 and b are the hydrostatic-pressure and shear DPs, respectively. In obtaining Equation (9.11), the SO split-off energy D0 is assumed to be D0 dEs. Introducing the InAs (x ¼ 0)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

285

values for aG0 , b and Cij (d ¼ 0.07) into Equation (9.11), we obtain the hydrostatic-pressure and shear-strain shifts dh and dEs in the strained InAs layer to be about 0.40 and 0.26 eV, respectively. Thus, the band-gap discontinuity between GaAs and fully strained InAs is DE0 ¼ E0 ðGaAsÞ½E0 ðInAsÞ þ dh 1:43ð0:36 þ 0:40Þ ¼ 0:67 eV

ð9:12Þ

Similarly, the discontinuity between GaAs and fully relaxed InAs is given by DE0 ¼ E0 ðGaAsÞE0 ðInAsÞ 1:430:36 ¼ 1:07 eV

ð9:13Þ

The InAs/GaAs heterostructure has about 7% lattice mismatch and the corresponding critical thickness is as low as two monolayers. Using XPS, Kowalczyk et al. [75] determined the band offsets in the InAs/GaAs(100) heterostructure to be DEc ¼ 0.90 0.07 eVand DEv ¼ 0.17 0.07 eV, respectively. The resulting offset ratio is DEc : DEv ¼ 16 : 84. The sample used by Kowalczyk et al. [75] was an InAs/GaAs(100) single heterojunction with a 20 A thick InAs layer, which is much thicker than the critical thickness for the generation of dislocation. Hence, the lattice strain is relaxed in their sample. In fact, the obtained band-gap discontinuity DE0 ¼ DEc þ DEv ¼ 1.07 eV exactly agrees with that predicted from Equation (9.13). If we assume an offset ratio of DEc : DEv ¼ 16 : 84 for the fully relaxed GaxIn1xAs/GaAs heterostructure, we can obtain the x-dependent offsets DEc and DEv (in eV) DEc ðxÞ ¼ 0:17x

ð9:14aÞ

DEv ðxÞ ¼ 0:90x

ð9:14bÞ

The largest d and DE0 values can be expected at x ¼ 0 for the strained GaxIn1xAs/GaAs heterostructure. Since both d and DE0 E0(GaAs) E0(GaxIn1xAs) for the strained GaxIn1xAs/GaAs heterostructure decrease almost linearly with increasing x, the hydrostatic component (dh) to DE0 ratio may be roughly independent of x and is given by dh/DE0 0.4 (0.40/1.07 at x ¼ 0). There are no experimental data on the band offsets in strained GaxIn1xAs/GaAs heterostructures for lower x values, except for x ¼ 0. Samples of larger x reported recently [27, 76–78] give a mean band-offset ratio of DEc : DEv ¼ 60 : 40 (0.6 < x 0.98). Using this ratio and the strained-InAs (x ¼ 0) E0 value, we can obtain an energy-band diagram for the strained GaxIn1xAs/GaAs heterostructure. This result is shown in Figure 9.10. The band offsets DEc,

ΔEc=0.48 eV GaAs GaAs (x=1.0) 0.63 eV

InAs (x=0) 0.76 eV 0.13 eV (HH-like) 0.13 eV (LH-like)

Ga In x

x 1-x

As/GaAs

ΔEv1=0.32 eV ΔEv2=0.06 eV

Figure 9.10 Schematic energy-band diagram for strained GaxIn1xAs/GaAs heterostructure obtained by using a band-offset ratio of DEc : DEv ¼ 60 : 40 and strained-InAs E0 value of 0.76 eV

286

PROPERTIES OF SEMICONDUCTOR ALLOYS

DEv1 (CB HH) and DEv2 (CB LH) versus x can be written as (in eV) DEc ðxÞ ¼ 0:48x

ð9:15aÞ

DEv1 ðxÞ ¼ 0:32x

ð9:15bÞ

DEv2 ðxÞ ¼ 0:06x

ð9:15cÞ

(e) Dilute-nitride-based heterostructure system 1. GaNAs/GaAs—Recent experimental studies suggest that the band lineup in the dilutenitride GaNxAs1x/GaAs heterostructure for N 4.5 at% is type I [79–83], although an earlier XPS study suggested a type-II lineup [84]. The schematic band diagram for this heterostructure system is shown in Figure 9.11. It is commonly accepted that N incorporation mainly affects the CB states and causes band-gap reduction (Section 6.3.5). Based on the BAC model, the N states produced in GaAs lead to a characteristic splitting of the G6-CB state into two non-parabolic subbands E and E þ (Figure 9.11(b), see also Figure 6.29(b)). The different lattice constants between c-GaN and GaAs can induce tensile strain parallel to [010] and [001] in pseudomorphic GaNxAs1x layers on GaAs(100) (Figure 1.27). This strain argument predicts that the LH band should be type I, while the HH band is type II, as illustrated in Figure 9.11(c). The CB offsets DEc ¼ (0.7 0.95)DEg were reported [79–83]. (a)

(b)

(c) E+

CB ΔE c

E-

ΔE v2(LH-like) VB GaAs

Ga N As x

1-x

ΔE v1 (HH-like) Ga N As x

1-x

GaAs

Figure 9.11 Schematic energy-band diagram for GaNxAs1x/GaAs heterostructure. Strain argument depicted in (c) predicts the LH and HH bands to be type I and type II, respectively

2. GaInNAs/GaAs—The schematic energy-band diagram for the dilute-nitride GaxIn1xNyAs1y/ GaAs heterostructure is shown in Figure 9.12. As mentioned in Section 9.1.4, the band-offset ratios in fully relaxed and strained GaxIn1xAs/GaAs heterostructures are assumed to be given by DEc : DEv ¼ 16 : 84 and 60 : 40, respectively. The band lineup in Figure 9.12(a) corresponds to the strained heterostructure. Strain-induced splitting of the HH and LH bands cannot be expected in the fully relaxed heterostructure system. Adding N to GaxIn1xAs splits the CB minimum into E and E þ and lowers the band-gap energy, with negligible interaction with the

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT (a)

287

(b) ΔE c

CB

E+ EΔEv1 (HH-like)

VB ΔEv2 (LH-like) GaAs

GalnAs

GalnNAs

Figure 9.12 Schematic energy-band diagrams for strained heterostructure systems: (a) GaxIn1xAs/ GaAs and (b) dilute-nitride GaxIn1xNyAs1y/GaAs

VB states (Figure 9.12(b)). We can, thus, expect an increase (decrease) in the DEc (DEv) portion. Indeed, the band discontinuities have been found to be 80% in the CB and 20% in the VB for GaxIn1xNyAs1y/GaAs heterostructures [85, 86]. 3. GaNAsSb/GaAs—As seen in Figure 9.11(b), incorporating N into GaAs essentially lowers the CB minimum. This is complementary to the Sb effect, which mainly increases the VB maximum. In this respect, the GaNxAsySb1xy/GaAs heterostructure is an interesting system where DEc and DEv can be independently tuned by adjusting N and Sb concentrations, respectively. The band discontinuities in this heterostructure system have been studied by several authors [87–90] and are found to change from type II to type I by incorporating N into GaAsxSb1x.

9.1.6 II–VI Semiconductor Heterostructure System (a) (II, II)–O-based heterostructure system The band alignment in the Mg0.15Zn0.85O/CdS heterostructure was studied using X-ray and UV photoelectron spectroscopy and found to be a staggered type-II alignment with electrons localized in the Mg0.15Zn0.85O layer (DEc ¼ 1.1 eV and DEv ¼ 1.2 eV) [91]. The XPS technique was used to obtain the band offsets in the Zn0.95Cd0.05O/ZnO(0001) heterostructure [92]. The band offsets obtained were DEc ¼ 0.30 eV and DEv ¼ 0.17 eV, with electrons and holes localized in the Zn0.95Cd0.05O layer (type I). (b) (II, II)S-based heterostructure system The band offsets in free-standing c-Zn0.7Cd0.3S/c-ZnS SL were determined from lowtemperature PL to be DEc ¼ 0.461 eV and DEv ¼ 0.088 eV (DEc : DEv ¼ 84 : 16) [93]. (c) (II, II)Se-based heterostructure system The band alignments in ZnSe-based heterostructures, such as BexZn1xSe/ZnSe, MgxZn1xSe/ ZnSe and ZnxCd1xSe/ZnSe, are type I. From magneto-transmission measurements on a series

288

PROPERTIES OF SEMICONDUCTOR ALLOYS

of BeZnSe/ZnMnSe QWs, Kim et al. [94] estimated the VB offset in BexZn1xSe/ZnSe to be approximately 40% of the band-gap difference. The VB offset in the MgxZn1xSe/ZnSe heterostructure was determined from optical and photoelectron spectra to be as much as 87% of the band-gap difference [95]. The band offsets in the ZnxCd1xSe/ZnSe heterostructure were determined using various techniques, such as optical absorption [96], reflectance [97], electrical conductivity and intersubband absorption [98], PLE [99] and CL and DLTS [100]. These data gave a band-offset ratio which varied from DEc : DEv ¼ 67 : 33 to 87 : 13. We obtained DEc : DEv ¼ 72 : 28 as the average band-offset ratio. Guenaud et al. [99] reported that the HH excitons are type I, whereas the LH excitons are type II. The type-II excitons were considered to occur as a result of the compressive strain state and to have small VB offset (DEc : DEv ¼ 87 : 13) in the ZnxCd1xSe/ZnSe (x ¼ 0.82 0.88) heterostructure. The band offsets in the ZnxCd1xSe/MgSe heterostructure have also been studied [101]. (d) (II, II)Te-based heterostructure system It is generally accepted that the strained ZnxCd1xTe/CdTe heterostructure is of mixed type, i.e. the electrons and heavy holes are confined in a CdTe layer, while the light holes are confined in a ZnxCd1xTe layer [102–105]. This is the result of sufficient residual tensile strain existing in the ZnxCd1xTe layer grown on ZnyCd1yTe (x > y). Similarly, band alignments of type I and type II have been observed in ZnxCd1xTe/ZnTe heterostructures below and above x 0.1 respectively, grown on GaAs(100) [106]. The electrons and holes in type II can be confined in the ZnxCd1xTe and ZnTe layers, respectively. The VB offset between CdTe and HgTe has been the subject of a number of investigations. In early experiments, both a small offset of 40 meV and a roughly 10 times larger value were deduced (see von Truchseb et al. [107]). However, more recent experiments using various techniques provide consistent VB offsets somewhere around 0.4 eV [108–113]. The most recent study gives temperature-dependent offset data of DEv ¼ 0.57 0.06 eV at 5 K and its temperature coefficient dDEv/dT 0.4 meV/K [114]. Strong evidence has also been provided to suggest that the temperature dependence of the band offsets can be essentially neglected [112]. Figure 9.13 shows the schematic band diagram for the CdxHg1xTe/CdTe heterostructure. The HgTe/CdTe lineup corresponds to that reported by Becker et al. [114]. The results

CdTe/CdTe

CdTe/CdxHg1-xTe

CdTe/HgTe

Γ6 Electron

Γ8

E0=1.51 eV

Hole

Γ8 x

ΔEc =1.21 eV

Γ6

E0 =-0.15 eV

ΔE v = 0.45 eV

Figure 9.13 Schematic energy-band diagram for CdxHg1xTe/CdTe heterostructure. The HgTe/CdTe lineup corresponds to that reported by Becker et al. [114] at 300 K. The band offsets can be written as Equation (9.16)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

289

suggest that the band offsets can be expressed as (in eV) DEc ðxÞ ¼ 1:211:21x

ð9:16aÞ

DEv ðxÞ ¼ 0:450:45x

ð9:16bÞ

Thus, the CdxHg1xTe/CdTe heterostructure is type II (x ¼ 0) and becomes type I for x > 0.09. (e) Zn(VI, VI)-based heterostructure system Shahzad et al. [115] carried out PL and PLE measurements on ZnSxSe1x/ZnSe SLs (x 0.26) and obtained a very small CB offset (10 meV) between ZnSe wells and ZnSxSe1x barriers with a type-I lineup. Subsequently, Lomascolo et al. [116] undertook PL measurements on a ZnS0.18Se0.82/ZnSe SL at hydrostatic pressures up to 8 GPa and confirmed a transition from type I to type II near 4.5 GPa. The CB offset estimated in this study was DEc 6 meV at zero pressure. We can thus conclude that the band-offset ratio for ZnSxSe1x/ZnSe heterostructure is roughly given by DEc : DEv ¼ 0 : 100. ZnSe/ZnTe is known to comprise a staggered type-II heterostructure. The same band alignment can be expected and has been confirmed in ZnSexTe1x/ZnSe and ZnSexTe1x/ZnTe heterostructures [117, 118]. (f) (II, II)VI-based and II(VI, VI)-based heterostructure systems The band offsets in MgZnSe/ZnCdSe and ZnCdSe/ZnSSe heterostructures were determined experimentally by Pelucchi et al. [119] and Wu et al. [120], respectively. (g) (II, II)(VI, VI)-based heterostructure system The band lineup for MgxZn1xSySe1y/ZnSe heterostructure is believed to be type I. The bandoffset ratio was studied experimentally by several authors [121–126]. These studies provided offset ratios which varied largely from DEc : DEv ¼ 10 : 90 [124] to 60 : 40 [122]. We obtained DEc : DEv ¼ 36 : 64 as the mean value. The band offsets in Zn0.7Cd0.3S0.06Se0.94/ZnS0.06Se0.94 lattice-matched to GaAs have been characterized by DLTS [127] and the band-offset ratio obtained was DEc : DEv ¼ 75 : 25. (h) (II, II, II)VI-based heterostructure system The band alignment in BexMgyZn1xySe/ZnSe grown on GaAs(100) was investigated using PL and PLE [128] and the band-offset ratio was found to be DEc : DEv ¼ 60 : 40. The band offsets in Mg0.50Zn0.27Cd0.23Se/Zn0.53Cd0.47Se lattice-matched to InP were investigated using contactless ER [129]; the offset ratio was determined to be DEc : DEv ¼ 82 : 18 (DEc ¼ 0.59 eV).

9.2 SCHOTTKY BARRIER HEIGHT 9.2.1 General Considerations A Schottky barrier is a metal/semiconductor junction which has rectifying characteristics. Rectifying properties depend both on the metal work function and type of conductivty of

290

PROPERTIES OF SEMICONDUCTOR ALLOYS

the semiconductor. The choice of a metal for fabricating the Schottky barrier with a particular semiconductor is, thus, determined by its electronic work function fM. For an n-type semiconductor, fM should be large, while for a p-type semiconductor, it should be less than the electron affinity xe of the semiconductor. The barrier heights can then be written, respectively, as n-type : fn ¼ fM xe

ð9:17aÞ

p-type : fp ¼ Eg fM þ x e

ð9:17bÞ

where Eg is the band-gap energy of the semiconductor. The maximum value of the barrier height for an ideal SchottkyMott contact is about equal to the band-gap energy of the semiconductor: fn þ fp ¼ Eg. The work functions fM of some important metals used as the Schottky contacts are summarized in Table 9.2 of Adachi [1].

9.2.2 Group-IV Semiconductor Alloy (a) SiGe binary alloy

0.9 0.8 0.7 0.6 0.5 0.4 0.7

1.2 Metal/SixGe1-x

(a)

(c) 1.1

φn+φp , EgX (eV)

φp (eV)

φn (eV)

Extended studies on metal/SixGe1x have shown the complexity of the mechanism of Schottky barrier formation [130]. The results are still puzzling. However, a common trend has been observed: the Schottky barrier height fp increases with increasing x. The experimental data for fn and fp obtained by Aubry-Fortuna et al. [130] is shown in Figure 9.14. These authors observed that for lower-fM metals (Zr and Ti), fn decreases with x, while fp increases. For a higher fM metal (Pt), fn greatly increased. In the intermediate-fM metal (W), fn exactly follows the increase of Eg in SixGe1x with x, while fp remains constant. Nevertheless, whatever the metal, the sum fn þ fp gives the Eg variation as a function of x (Equation (9.17)), and the Fermi level is located at the same position for both n- and p-type layers. Figure 9.14(c)

Lower-φM Intermediate-φM Higher-φM

0.6 0.5 0.4 0.3 0.4

1.0 0.9 0.8

EgX

(b) 0.5

φn+φp (lower-φM)

0.6

0.7 x

0.8

0.9

1.0

0.7 0.4 0.5 0.6 0.7 0.8 0.9 1.0 x

Figure 9.14 Schottky barrier heights (a) fn and (b) fp for metal/SixGe1x contacts. The experimental data are taken from Aubry-Fortuna et al. [130]. The sum fn þ fp for the lower-fM metals, together with the band-gap energy EgX (Figure 6.8), are plotted against x in (c)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

291

shows a comparison of the sum fn þ fp for the lower-fM metals plotted in Figures 9.14(a) and 9.14(b) with the variation in EgX with x in SixGe1x (Figure 6.8). As for metal/Si and metal/Ge contacts [1], the results in Figure 9.14(c) suggest that the Schottky barrier height for metal/ SixGe1x contact exhibits the SchottkyMott contact nature very well. (b) CSiGe ternary alloy The Schottky barrier height on CxSiyGe1xy has been studied by several authors [130]. Adding C to SiGe leads to an increase in the W or Ti/p-type Schottky barrier height which is larger than that of the band-gap energy Eg, showing a change in the Fermi level position. Nevertheless, as in the case of SixGe1x, a weaker dependence on fM compared to that of Si is observed. High values of the ideality factor with increasing C content have also been observed.

9.2.3 III–V Semiconductor Ternary Alloy (a) (III, III) N alloy The Schottky rectifier properties of n-AlxGa1xN have been studied using various metal contacts. The Schottky barrier height fn versus x obtained by depositing Au, Ni and Pd metals on n-AlxGa1xN is shown in Figure 9.15. The experimental data are taken from various sources [131–135]. These plots suggest that it is difficult to establish an ideal Schottky contact and, thus, to obtain simple relationships such as that shown in Equation (9.17). This may be due to interface states caused by surface reactions of metal and semiconductor atoms and/or to any effects of crystalline imperfection. The n-AlxGa1xN samples plotted in Figure 9.15 were epitaxially grown on sapphire [131, 132, 134, 135] or on 6H-SiC substrate [133]. 1.8

1.8 (a) I-V

(b) C-V Au Ni Pd

1.4

1.6

φn (eV)

φn (eV)

1.6

1.2

1.4 1.2

1.0

1.0

0.8

0.8

0.6

0

0.1

0.2 x

0.3

0.6

Metal/AlxGa1-xN

0

0.1

0.2

0.3

x

Figure 9.15 Schottky barrier height fn versus x for samples with Au, Ni and Pd metals deposited on nAlxGa1xN: (a) I Vand (b) C V measurements. The experimental data are taken from various sources (see text)

Zhang et al. [136] reported the x-dependent breakdown voltage in an n-AlxGa1xN Schottky rectifier. The breakdown voltage increased from 2.3 kV for x ¼ 0 (GaN) to 4.3 kV for x ¼ 0.25. They also demonstrated that the use of p þ guard rings is effective in preventing premature edge breakdown.

292

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b) (III, III)P alloy

1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

3.0 (a)

2.7

(c)

2.4

φn+φp , Eg (eV)

φp (eV)

φn (eV)

Figure 9.16 shows the experimental fn and fp values for Au/GaxIn1xP Schottky barriers obtained by several authors [137–139]. The GaP and InP values are taken from Adachi [1]. The barrier height fn in Figure 9.16(a) increases almost linearly with increasing x, while fp in Figure 9.16(b) shows no strong dependence on x. The sum of fn and fp, together with E0 and EgX , are plotted against x in Figure 9.16(c). The Au/GaxIn1xP rectifiers show Schottky– Mott-like characteristics.

Au/GaxIn1-xP

E Xg

2.1 1.8 1.5

E0

1.2

0

φn+φp

0.9

(b) 0.2

0.4

x

0.6

0.8

1.0

0.6 0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.16 Schottky barrier heights (a) fn and (b) fp for Au/GaxIn1xP contacts. The experimental data are taken from various sources (see text). The open squares in (a) and (b) represent the endpoint binary data in Adachi [1]. The sum fn þ fp, together with E0 and EgX (Table 6.10), are plotted against x in (c)

The Schottky barrier heights for the common III–V and II–VI semiconductors allow a pattern in which the barrier height of p-type semiconductors (fp) can be determined solely by the anion of the semiconductor [140]. The corresponding barrier height of n-type semiconductors (fn) may be determined from the relationship of fn þ fp ¼ Eg. Hence, the difference in the barrier heights of the two n-type semiconductors with the same anion is equal to the difference in the band-gap energies between them. In Figure 9.16(b), we can see that the Au/ GaxIn1xP system obeys this rule, namely, the ‘common anion’ rule. The dependence of x on the Schottky barrier height fn for Ti/Pt/Au metals on AlxIn1xP (0 < x < 0.5) has been studied using IV and CV measurements [141]. The results obtained suggest that fn increases almost linearly with x at a rate of 14 meV/at%[Al]. This value is slightly smaller than that of E0, 22 meV/at%[Al] (Table 6.9). Thus, the metal/AlxIn1xP system may not obey the common anion rule (i.e. fp is dependent of x). (c) (III, III)As alloy 1. AlGaAs—The fn and fp values as a function of x for Al/AlxGa1xAs Schottky system have been plotted in Figure 9.17. The experimental data are taken from Adachi [26]. The solid lines in Figures 9.17(a) and 9.17(b) show the linear fits of these data (in eV) fn ðxÞ ¼ 0:77 þ 0:84x ð0 x 0:425Þ

ð9:18aÞ

fn ðxÞ ¼ 1:220:22x ð0:45 < x 1:0Þ

ð9:18bÞ

1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

293

3.0 φn+φp

2.7

E0, EgX

φn+φp , Eg (eV)

φp (eV)

φn (eV)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

Al/AlxGa1-xAs

(a)

(b)

2.4 2.1

X

Eg

1.8 E0

1.5

I-V C-V

0

0.2

0.4

0.6

0.8

1.2 0

1.0

x

(c) 0.2 0.4 0.6 0.8 1.0 x

Figure 9.17 Schottky barrier heights (a) fn and (b) fp for Al/AlxGa1xAs contacts. The experimental data are taken from Adachi [26]. The solid lines in (a) and (b) show the linear least-squares fits of Equation (9.18). The sum fn þ fp, together with E0 and EgX (Table 6.11), are plotted against x in (c)

fp ðxÞ ¼ 0:64 þ 0:52x

ð9:18cÞ

It can be easily seen from Equation 9.18(c) that the Al/AlxGa1xAs system does not obey the common anion rule. However, the sum of fn and fp plotted in Figure 9.17(c) is almost equal to the fundamental absorption edge E0 (or EgX ). The x-dependent Schottky barrier heights fn and fp in Figure 9.17 resemble those of the CB and VB offsets (DEc, DEv) shown in Figure 9.5. Tersoff [142] pointed out that the band lineups at semiconductor heterojunctions are simply correlated with the difference in the Schottky barrier heights formed by using the same metal on the semiconductors of the heterojunction pair. In essence, this means that the physical mechanism responsible for determining the Fermi level in Schottky barrier formation also determines the band lineups in heterostructures. 2. AlInAs—Figure 9.18 shows the fn and fp values plotted as a function of x for Al/AlxIn1xAs Schottky system. The experimental data are taken from various sources [143–145]. 3.0 φn+φp

(a)

φn (eV)

2.4

φn+φp , Eg (eV)

1.8 1.5 1.2 0.9 0.6 0.3 0 -0.3 1.8 1.5 1.2 0.9 0.6 0.3 0

φp (eV)

(b)

1.2

0.4

0.6 x

0.8

E0

(c)

Al/AlxIn1-xAs 0.2

EgX

1.8

0.6

0

X

E0, Eg

1.0

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.18 Schottky barrier heights (a) fn and (b) fp for Al/AlxIn1xAs contacts. The sum fn þ fp, together with E0 and EgX (see Table 6.13), are plotted against x in (c)

294

PROPERTIES OF SEMICONDUCTOR ALLOYS

The AlAs and InAs data are obtained from Adachi [146]. No experimental data has been reported for the Al/p-InAs Schottky barrier height (fp). In Figure 9.18(b), therefore, we plot the experimental fp for Au/p-InAs contact [146]. It should be noted that any metal/n-InAs (x ¼ 1.0) contact usually shows Ohmic behavior (i.e. fn 0 eV) [146]. The fp versus x plots in Figure 9.18(b) suggest that the Al/AlxIn1xAs system does not obey the common anion rule. However, the simple relationship fn þ fp E0ðEgX Þ holds in Figure 9.18(c). 3. GaInAs—The Schottky barrier height fn for Au/GaxIn1xAs contact has been determined using IV and CV measurements [147]. Figure 9.19 shows the results of these 1.2

φn (eV)

0.9

Au/GaxIn1-xAs

0.6 0.3 0 Ohmic

-0.3 0

0.2

0.4

0.6

0.8

1.0

x

Figure 9.19 Schottky barrier height fn for Au/GaxIn1xAs contact. The experimental data are taken from Adachi [1] (open squares) and Kajiyama et al. [147] (solid circles). The solid line shows the quadratic least-squares fit of Equation (9.19). The negative fn sign for x 0.15 indicates the downward bending of the CB at the interface (Ohmic contact)

measurements. The solid line represents the quadratic least-squares fit of the experimental data (in eV) fn ¼ 0:03 þ 0:05x þ 0:95x2 ð9:19Þ The Au/GaxIn1xAs contact is predicted to be Ohmic for x 0.15 (fn 0 eV). The negative fn sign stands for the downward bending of the CB at the interface. A Schottky barrier height of fn 0.2 eV is predicted for metal/n-Ga0.47In0.53As latticematched to InP. The barrier height control is an important tool in fabricating various devices. Diode engineered for high barrier height systematically showed a higher thermal stability than low-barrier diodes. Many attempts have therefore been made to enhance the barrier height of n-GaxIn1xAs by inserting various thin interlayers between the metal and n-GaxIn1xAs layer. Such interlayers were counter-doped p þ -GaxIn1xAs, n-InP, p-InP, n-GaAs, n-GaxIn1xP at different thickness and dopant densities, etc. [148, 149]. An effective barrier height up to fn 0.7 eV has been achieved. (d) (III, III)Sb alloy Figures 9.20(a) and 9.20(b) show the Shottky barrier height fn for Au/AlxGa1xSb and Au/ GaxIn1xSb contacts, respectively. The experimental data are taken from Chin et al. [150] and Keeler et al. [151], respectively. The solid line in Figure 9.20(a) shows the linear least-squares fit of the experimental data and provides fn 1.02 eV for Au/AlSb (x ¼ 1.0) contact. The

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT 1.2

1.2 (a) Au/AlxGa1-xSb

(b) Au/GaxIn1-xSb 0.9

φn (eV)

φn (eV)

0.9

0.6

0.3

0

295

0.6

0.3

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.20 Schottky barrier height fn for (a) Au/AlxGa1xSb and (b) Au/GaxIn1xSb contacts. The experimental data in (a) are taken from Chin et al. [150] and in (b) from Keeler et al. [151]. The open squares in (a) and (b) represent the endpoint binary data taken from Adachi [1]. The solid line in (a) shows the linear least-squares fit and estimates fn 1.02 eV for Au/AlSb contact

barrier height fp for Au/AlSb is 0.56 eV [1]. The sum fn þ fp 1.58 eV for Au/AlSb contact is, thus, slightly smaller than the AlSb band-gap energy EgX ¼ 1:615 eV (Table 6.1). The Schottky barrier height for Au/GaxIn1xSb can be expected to be fp 0 eV (i.e. Ohmic) [1]. Note, however, that Keeler et al. [151] obtained 0.017 fp 0.022 eV for Au contacts on p-GaxIn1xSb (0.62 x 0.905) layers. (e) Ga(V, V) alloy GaP0.35Sb0.65 is an InP lattice-matched material. In order to overcome the low value of the Schottky barrier height on n-InP (fn 0.4 eV [1, 146]), Loualiche et al. [152] fabricated a Au/ GaP0.35Sb0.65 Schottky barrier on InP and obtained a value of fn 0.6 eV. This value is the highest ever reported on InP lattice-matched materials that do not contain aluminum. The Schottky barrier height fn for Au/GaAsxSb1x contact has been determined using I–V and C–V measurements [153]. Figure 9.21 shows these results, together with the x dependence

1.8

1.8 1.5

Au/GaAsxSb1-x

1.2

1.2 E0

0.9 0.6

0.6

φn

0.3 0

0.9

0

0.2

0.4

x

0.6

E0 (eV)

φn (eV)

1.5

0.3 0.8

0 1.0

Figure 9.21 Schottky barrier height fn for Au/GaAsxSb1x contact, together with E0 for GaAsxSb1x (Table 6.23). The experimental data are obtained from Zhao et al. [153]. The open squares represent the endpoint binary data taken from Adachi [1]

296

PROPERTIES OF SEMICONDUCTOR ALLOYS

of E0 (Table 6.23). The solid line represents the quadratic least-squares fit given by (in eV) fn ðxÞ ¼ 0:680:88x þ 1:11x2

ð9:20Þ

We can see that both E0 and fn show a remarkable nonlinearly with respect to x.

9.2.4 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) alloy

1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

2.2 (a)

φn+φp

2.0 I-V C-V

φn+φp , E0 (eV)

φp (eV)

φn (eV)

1. GaInPAs—We show in Figure 9.22 the Schottky barrier heights fn and fp as a function of y for Au metal on GaxIn1xPyAs1y/GaAs. The sum of fn and fp, together with E0 (Table 6.28), are also plotted against y. The experimental data are taken from Lee et al. [154] and Sugino and Kousaka [155]. The Au metal on GaxIn1xPyAs1y/GaAs exhibits the SchottkyMott barrier characteristics satisfactorily (Equation (9.17)).

(b)

1.8 1.6 1.4 1.2

Au on GaxIn1-xPyAs1-x/GaAs 0

0.2

0.4

0.6

0.8

1.0

E0

1.0 0

y

(c) 0.2 0.4 0.6 0.8 1.0 y

Figure 9.22 Schottky barrier heights (a) fn and (b) fp for Au on GaxIn1xPyAs1y/GaAs. The sum fn þ fp, together with E0 (Table 6.28), are plotted against y in (c). The experimental data in (a)-(c) are taken from Lee et al. [154] and Sugino and Kousaka [155]

The Schottky barrier properties of Au metal on GaxIn1xPyAs1y/InP are shown in Figure 9.23. The fn data are taken from Morgan et al. [156] and Bhattacharya and Yeaman [157], while those for fp are from Escher et al. [158]. The solid lines represent the linear least-squares fits (in eV) fn ðxÞ ¼ 0:20 þ 0:44y

ð9:21aÞ

fp ðxÞ ¼ 0:47 þ 0:30y

ð9:21bÞ

The heavy solid line in Figure 9.23(c) shows the sum of these values against y. 2. AlGaAsSb and GaInAsSb—The Schottky barrier heights for Au, Al and Sb metals on n- and p-Al0.5Ga0.5As0.05Sb0.95/GaSb layers were studied by Polyakov et al. [159]. These authors

1.0 0.8 0.6 0.4 0.2 0 1 0.8 0.6 0.4 0.2 0

297

1.6 (a)

(c) 1.4

φn+φp , E0 (eV)

φp (eV)

φn (eV)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

(b)

0.2

0.4

0.6

0.8

1.2 1.0 E0

0.8 0.6

Au on GaxIn1-xPyAs1-y /InP 0

φn+φp

1.0

0.4 0

y

0.2 0.4 0.6 0.8 1.0 y

Figure 9.23 Schottky barrier heights (a) fn and (b) fp for Au on GaxIn1xPyAs1y/InP. The experimental data in (a) are taken from Morgan et al. [156] and Bhattacharya and Yeaman [157] and in (b) from Escher et al. [158]. The open circle is taken from Figure 9.19. The solid lines in (a) and (b) show the linear least-squares fits of Equation (9.21). The sum of fn and fp, together with E0 (Table 6.28), are plotted against y in (c)

found that the Schottky barriers are high for Au (1.3 eV) and Al (1.2 eV) on n-type material and very low on p-type materials. The behavior of Sb was unique with fn,p being 0.6–0.7 eV. The reason for the surface location of the Fermi-level pinning due to Au and Al metals may be related to a predominance of Ga-antisite-type native acceptors at the surface, which is not the case for Sb metal. The Schottky barriers for Al, Au and Sb metals on n-GaxIn1xAsySb1y/GaSb (x ¼ 0.85) were determined by Polyakov et al. [160]. All these Schottky barriers had heights of 0.5 eV, with the surface Fermi level located at Ev þ 0.16 eV. (b) (III, III, III)V alloy 1. AlGaInN—Figure 9.24 plots the fn versus x for Pd/AlxGa0.98xIn0.02N contact obtained from I V and C V measurements [161]. The alloy samples were grown on (0001)sapphire substrates by MOCVD. It was found that the larger difference in fn between IV 2.4 Pd/AlxGa0.98-xIn0.02N

φn (eV)

2.1 1.8

I-V C-V

1.5 1.2 0.9 0.6

0

0.1

0.2

0.3

x

Figure 9.24 Schottky barrier height fn for Pd/AlxGa0.98xIn0.02N contact obtained by Liu et al. [161]

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

3.0 2.7 2.4

φn+φp , Eg (eV)

φp (eV)

φn (eV)

298

(a)

(b)

2.1

E0

1.8 1.5 1.2 0.9

φn+φp

0.6 Au on (AlxGa1-x)0.53In0.47P/GaAs

0

0.2

0.4

0.6

0.8

0.3 0 0

1.0

EgX

x

(c) 0.2 0.4 0.6 0.8 1.0 x

Figure 9.25 Schottky barrier heights (a) fn and (b) fp for Au on (AlxGa1x)0.53In0.47P/GaAs. The sum of fn and fp, together with E0 and EgX (Table 6.28), are plotted against x in (c). The experimental data are taken from Nanda et al. [137] (solid circles) and Wang et al. [162] (open circles)

and C V measurements could not be quantitatively explained by the traditional electron transport mechanisms of the Schottky barrier rectifier, such as the tunneling effect, imageforce effect or barrier inhomogeneity theory. 2. AlGaInP—The Schottky barrier heights fn and fp for Au metal on (AlxGa1x)0.53In0.47P/ GaAs are shown in Figure 9.25. The experimental data are taken from Nanda et al. [137] (solid circles) and Wang et al. [162] (open circles). The unique feature of this rectifying contact system is that both fn and fp show no strong dependence on alloy composition. If we accept the common anion rule, no strong x dependence of fp can be expected. In Figure 9.25(c), the sum of fn and fp obtained by Nanda et al. [137], together with E0 and EgX (Table 6.28), are plotted against composition x. It is apparent that fn þ fp „ E0 (or EgX ) for this rectifying contact system. 3. AlGaInAs—The Schottky barrier height fn for Au metal on (AlxGa1x)0.48In0.52As/InP has been obtained using IV and CV measurements [163]. These results are plotted in Figure 9.26. The ideality factors determined from the forward-bias IV characteristics were 0.8 Au/(AlxGa1-x)0.48In0.52As

φn (eV)

0.6 0.4 0.2 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 9.26 Schottky barrier height fn for Au on (AlxGa1x)0.48In0.52As/InP. The experimental data are taken from Schramm et al. [163]. The data represented by the open circle is taken from Figure 9.19. The solid line shows the linear least-squares fit of Equation (9.22)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

299

in the range 1.08 1.2, indicating that the Schottky contacts were of high quality. The open circle represents the Au/Ga0.47In0.53As barrier height taken from Figure 9.19. The solid line shows the linear least-squares fit of these data (in eV) fn ðxÞ ¼ 0:20 þ 0:37x

ð9:22Þ

9.2.5 II–VI Semiconductor Alloy (a) (II, II)Te ternary alloy The Schottky barrier height fp for In metal on MgxZn1xTe determined by CV and photoelectron measurements [164] is plotted in Figure 9.27(a). The solid line shows the linear least-squares fit of these data (solid circles). This fit predicts a negative fp value of 0.36 eV (Ohmic contact) for x ¼ 1.0 (MgTe). The open circle also represents the In/pZnTe data in Adachi [165]. The dashed line corresponds to the common anion rule, fp ¼ 1.06 eV. Using this fp value and assuming ideal Schottky–Mott contact, we can estimate fn 1.4 and 1.2 eV for In/n-MgTe and In/n-ZnTe contacts, respectively. 3.6

3.0

(a) In/Mgx Zn1-xTe

(b) Au/Zn xCd1-xTe 2.4

2.4

E0

EgX

1.8 φp

1.2

Common anion rule

φp, E0 (eV)

φp, Eg (eV)

3.0

E0

1.8 1.2

φp

0.6

0.6

Common anion rule

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.27 (a) Schottky barrier height fp for In/MgxZn1xTe contact, together with E0 and EgX (Figure 6.58). The experimental data are taken from Akkad et al. [164]. The solid line shows the linear least-squares fit. The open circle represents the In/ZnTe data taken from Adachi [165]. The dashed line indicates the common anion rule (fp ¼ 1.06 eV). (b) Schottky barrier height fp for Au/ZnxCd1xTe contact (see text), together with E0 for ZnxCd1xTe (Table 6.30). The open circles show the Au/ZnTe and Au/CdTe data [1, 165]. The dashed line indicates the common anion rule (fp ¼ 0.6 eV)

The Schottky barrier height fp for Au metal on ZnxCd1xTe is plotted against x in Figure 9.27(b). The experimental data are taken from various sources [166–168]. These data scatter largely and fall within fp ¼ 1.0 0.4 eV (0 < x < 0.2). The open circles also show the Au/p-ZnTe and Au/p-CdTe data in Adachi [1, 165]. Using the common anion rule (fp ¼ 0.6 eV, dashed line) and assuming ideal Schottky–Mott contact, we obtain fn 1.7 and 0.9 eV for Au/n-ZnTe and Au/n-CdTe contacts, respectively. The fn value reported for Au/n-CdTe in the literature is 0.59–1.0 eV [1, 165]. No fn value has been reported for any metal/n-ZnTe contact.

300

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b) Zn(VI, VI) ternary alloy ZnSxSe1x can be grown lattice-matched to GaAs (x ¼ 0.06–0.07). The Schottky contacts were formed on n-ZnS0.07Se0.93 epilayers grown on n-GaAs by MBE for metals with different work functions, Yb, Al, Cr, Cu, Au and Pd [169]. The fn value for Au/n-ZnS0.07Se0.93 contact has been plotted in Figure 9.28. The open circles represent the Au/n-ZnS and Au/n-ZnSe data taken from Adachi [1, 165]. The solid line also shows the linearly interpolated result between the endpoint binary data (in eV) fn ðxÞ ¼ 1:45 þ 0:65x

ð9:23Þ

4.2

φn, E0 (eV)

3.6

E0

3.0 2.4

φn

1.8 1.2

Au/ZnSxSe1-x

0.6 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 9.28 Schottky barrier height fn for Au/ZnSxSe1x contact, together with E0 for ZnSxSe1x (Table 6.30). The experimental data (x ¼ 0.07) is taken from Wang et al. [169]. The open circles show the Au/ZnS and Au/ZnSe data taken from Adachi [1, 165]. The solid line indicates the linearly interpolated result given by Equation (9.23)

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] K. Brunner, K. Eberl, and W. Winter, Phys. Rev. Lett. 76, 303 (1996). [3] A. A. Demkov and O. F. Sankey, Phys. Rev. B 48, 2207 (1993). [4] D. C. Houghton, G. C. Aers, N. L. Rowell, K. Brunner, W. Winter, K. Eberl, Phys. Rev. Lett. 78, 2441 (1997). [5] R. L. Williams, G. C. Aers, N. L. Rowell, K. Brunner, W. Winter, and K. Eberl, Appl. Phys. Lett. 72, 1320 (1998). [6] S. H. Ke, T. Uda, and K. Terakura, Phys. Rev. B 59, 15013 (1999). [7] G. N. Northrop, J. F. Morar, D. J. Wolford, and J. A. Bradley, J. Vac. Sci. Technol. B 10, 2018 (1992). [8] S. Fukatsu and Y. Shiraki, Appl. Phys. Lett. 63, 2378 (1993). [9] M. Wachter, K. Thonke, and R. Sauer, Thin Solid Films 222, 10 (1992). [10] T. Bajer, U. Mantz, K. Thonke, R. Sauer, F. Sch€affler, H. -J. Herzog, Phys. Rev. B 50, 15191 (1994). [11] M. L. W. Thewalt, D. A. Harrison, C. F. Reinhart, J. A. Wolk, and H. Lafontaine, Phys. Rev. Lett. 79, 269 (1997). [12] H. H. Cheng, S. T. Yen, and R. J. Nicholas, Phys. Rev. B 62, 4638 (2000). [13] B. L. Stein, E. T. Yu, E. T. Croke, A. T. Hunter, T. Laursen, A. E. Bair, J. W. Mayer, and C. C. Ahn, Appl. Phys. Lett. 70, 3413 (1997).

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

301

[14] B. L. Stein, E. T. Yu, E. T. Croke, A. T. Hunter, T. Laursen, J. W. Mayer, and C. C. Ahn, J. Vac. Sci. Technol. B 16, 1639 (1998). [15] R. Hartmann, U. Gennser, H. Sigg, D. Gr€utzmacher, and K. Ensslin, Appl. Phys. Lett. 73, 1257 (1998). [16] J. Kolodzey, F. Chen, B. A. Orner, D. Guerin, and S. I. Shah, Thin Solid Films 302, 201 (1997). [17] Y. Zhang, A. Mascarenhas, and L.-W. Wang, Appl. Phys. Lett. 80, 3111, (2002), and references cited therein. [18] D. Patel, M. J. Hafich, G. Y. Robinson, and C. S. Menoni, Phys. Rev. B 48, 18031 (1993). [19] M. D. Dawson, S. P. Najda, A. H. Kean, G. Duggan, D. J. Mowbray, O. P. Kowalski, M. S. Skolnick, and M. Hopkinson, Phys. Rev. B 50, 11190 (1994). [20] I.-J. Kim, Y.-H. Cho, K.-S. Kim, B.-D. Choe, and H. Lim, Appl. Phys. Lett. 68, 3488 (1996). [21] R. Dingle, W. Wiegmann, and C. H. Henry, Phys. Rev. Lett. 33, 827 (1974). [22] R. Dingle, A. C. Gossard, and W. Wiegmann, Phys. Rev. Lett. 34, 1327 (1975). [23] R. C. Miller, A. C. Gossard, D. A. Kleinman, and O. Munteanu, Phys. Rev. B 29, 3740 (1984). [24] R. C. Miller, D. A. Kleinman, and A. C. Gossard, Phys. Rev. B 29, 7085 (1984). [25] G. Duggan, H. I. Ralph, and K. J. Moore, Phys. Rev. B 32, 8395 (1985). [26] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, (1994). [27] S. Adachi, in Properties of Lattice-matched and Strained Indium Gallium Arsenide, EMIS Datareviews Series No. 8 (edited by P. Bhattacharya), INSPEC, London, 1993, p. 84. [28] J. B€ohrer, A. Krost, T. Wolf, and D. Bimberg, Phys. Rev. B 47, 6439 (1993). [29] E. Lugagne-Delpon, J. P. Andre, and P. Voisin, Solid State Commun. 86, 1 (1993). [30] W. Seidel, O. Krebs, P. Voisin, J. C. Harmand, F. Aristone, and J. F. Palmier, Phys. Rev. B 55, 2274 (1997). [31] J. P. Landesman, J. C. Garcia, J. Massies, P. Maurel, G. Jezequel, J. P. Hirtz, and P. Alnot, Appl. Phys. Lett. 60, 1241 (1992). [32] J. M. Lopez-Villegas P. Roura, J. Bosch, J. R. Morante, A. Georgakilas, and K. Zekentes, J. Electrochem. Soc. 140, 1492 (1993). [33] J.-H. Huang and T. Y. Chang, J. Appl. Phys. 76, 2893 (1994). [34] K. Tanaka, N. Kotera, and H. Nakamura, J. Appl. Phys. 85, 4071 (1999). [35] A. K. Srivastava, J. L. Zyskind, R. M. Lum, B. V. Dutt, and J. K. Klingert, Appl. Phys. Lett. 49, 41 (1986). [36] M. Mebarki, A. Kadri, and H. Mani, Solid State Commun. 72, 795 (1989). [37] S. S. Kizhaev, S. S. Molchanov, N. V. Zotova, E. A. Grebenshchikova, Y. P. Yakovlev, E. Hulicius, T. simecek, K. Melichar, and J. Pangrac, Tech. Phys. Lett. 27, 964 (2001). [38] H. A. Kaci, D. Boukredimi, and M. Mebarki, Phys. Status Solidi A 163, 101 (1997). [39] O. Ostinelli, G. Almuneau, and W. B€achtold, Semicond. Sci. Technol. 21, 681 (2006). [40] J. S. Nelson, S. R. Kurtz, L. R. Dawson, and J. A. Lott, Appl. Phys. Lett. 57, 578 (1990). [41] M. P. Mikhailova and A. N. Titkov, Semicond. Sci. Technol. 9, 1279 (1994). [42] M. A. Afrailov, A. N. Baranov, A. P. Dmitriev, M. P. Mikhailova, Y. P. Smorchkova, I. N. Timchenko, V. V. Sherstnev, Y. P. Yakovlev, and I. N. Yassievich, Sov. Phys. Semicond. 24, 876 (1990). [43] M. Mebarki, D. Boukredimi, and S. Sadik, J. L. Lazzari, J. Appl. Phys. 73, 2360 (1993). [44] J. R. Chang, Y. K. Su, and Y. T. Lu, J. Appl. Phys. 86, 6908 (1999). [45] M. P. Mikhailova, K. D. Moiseev, T. I. Voronina, T. S. Lagunova, and Y. P. Yakovlev, Semicond. 41, 161 (2007). [46] W. Z. Shen, S. C. Shen, W. G. Tang, Y. Chang, Y. Zhao, and A. Z. Li, J. Phys.: Condens. Matter 8, 4751 (1996). [47] J. R. Chang, Y. K. Su, C. L. Lin, K. M. Wu, W. C. Huang, Y. T. Lu, D. H. Jaw, and W. L. Li, S. M. Chen, Appl. Phys. Lett. 75, 238 (1999). [48] Y. Ishitani, E. Nomoto, T. Tanaka, and S. Minagawa, J. Appl. Phys. 81, 1763 (1997).

302

PROPERTIES OF SEMICONDUCTOR ALLOYS

[49] C. T. H. F. Liedenbaum, A. Valster, A. L. G. J. Severens, G. W. ‘t Hooft, Appl. Phys. Lett. 57, 2698 (1990). [50] O. P. Kowalski, J. W. Cockburn, D. M. Mowbray, M. S. Skolnick, R. Teissier, and M. Hopkinson, Appl. Phys. Lett. 66, 619 (1995). [51] H. K. Yow, P. A. Houston, and M. Hopkinson, Appl. Phys. Lett. 66, 2852 (1995). [52] A. D. Prins, J. L. Sly, A. T. Meney, D. J. Dunstan, Oreilly E. P. A. R. Adams, and A. Valster, J. Phys. Chem. Solids 56, 423 (1995). [53] T. M. Ritter, B. A. Weinstein, R. E. Viturro, and D. P. Bour, Phys. Status Solidi B 211, 869 (1999). [54] M. D. Dawson, G. Duggan, and D. J. Arent, Phys. Rev. B 51, 17660 (1995). [55] D. Vignaud and F. Mollot, J. Appl. Phys. 93, 384 (2003). [56] J. Shao, A. D€ornen, R. Winterhoff, and F. Scholz, Phys. Rev. B 66, 035109 (2002). [57] Y. Sugiyama, T. Inata, T. Fujii, Y. Nakata, S. Muto, and S. Hiyamizu, Jpn. J. Appl. Phys. 25, L648 (1986). [58] A. Sandhu, Y. Nakata, S. Sasa, K. Kodama, and S. Hiyamizu, Jpn. J. Appl. Phys. 26, 1709 (1987). [59] G. Martin, S. Strite, A. Botchkarev, A. Agarwal, A. Rockett, H. Morkoc, W. R. L. Lambrecht, and B. Segall, Appl. Phys. Lett. 65, 610 (1994). [60] J. Baur, K. Maier, M. Kunzer, U. Kaufmann, and J. Schneider, Appl. Phys. Lett. 65, 2211 (1994). [61] J. R. Waldrop and R. W. Grant, Appl. Phys. Lett. 68, 2879 (1996). [62] K. B. Nam, J. Li, K. H. Kim, J. Y. Lin, and H. X. Jiang, Appl. Phys. Lett. 78, 3690 (2001). [63] D. R. Hang, C. H. Chen, Y. F. Chen, H. X. Jiang, and J. Y. Lin, J. Appl. Phys. 90, 1887 (2001). [64] C. T. Foxon, S. V. Novikov, L. X. Zhao, and I. Harrison, Appl. Phys. Lett. 83, 1166 (2003). [65] A. N. Westmeyer, S. Mahajan, K. K. Bajaj, J. Y. Lin, H. X. Jiang, D. D. Koleske, and R. T. Senger, J. Appl. Phys. 99, 013705 (2006). [66] S. W. King, C. Ronning, R. F. Davis, M. C. Benjamin, and R. J. Nemanich, J. Appl. Phys. 84, 2086 (1998). [67] F. Bernardini, and V. Fiorentini, Phys. Rev. B 57, R9427 (1998). [68] C. -L. Wu, C. -H. Shen, and S. Gwo, Appl. Phys. Lett. 88, 032105 (2006). [69] P. D. C. King, T. D. Veal, P. H. Hefferson, C. F. McConville, T. Wang, P. J. Parbrook, H. Lu, and W. J. Schaff, Appl. Phys. Lett. 90, 132105 (2007). [70] C. Manz, M. Kunzer, H. Obloh, A. Ramakrishnan, and U. Kaufmann, Appl. Phys. Lett. 74, 3993 (1999). [71] H. Zhang, E. J. Miller, E. T. Yu, C. Poblenz, and J. S. Speck, Appl. Phys. Lett. 84, 4644 (2004). [72] C. -F. Shin, N. -C. Chen, P. -H. Chang, and K. -S. Liu, Jpn. J. Appl. Phys. 44, 7892 (2005). [73] T. Ohashi, P. Holmstr€om, A. Kikuchi, and K. Kishino, Appl. Phys. Lett. 89, 041907 (2006). [74] Z. H. Mahmood, A. P. Shah, A. Kadir, M. R. Gokhale, S. Ghosh, A. Bhattacharya, and B. M. Arora, Appl. Phys. Lett. 91, 152108 (2007). [75] S. P. Kowalczyk, W. J. Schaffer, E. A. Kraut, and R. W. Grant, J. Vac. Sci. Technol. 20, 705 (1992). [76] V. D. Kulakovskii, T. G. Andersson, and L. V. Butov, Semicond. Sci. Technol. 8, 477 (1993). [77] W. S. Chi, and Y. S. Huang, Semicond. Sci. Technol. 10, 127 (1995). [78] L. Lu, J. Wang, Y. Wang, W. Ge, G. Yang, and Z. Wang, J. Appl. Phys. 83, 2093 (1998). [79] Y. Zhang, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 61, 7479 (2000). [80] I. A. Buyanova, G. Pozina, P. N. Hai, W. M. Chen, H. P. Xin, and C. W. Tu, Phys. Rev. B 63, 033303 (2000). [81] P. Krispin, S. G. Spruytte, J. S. Harris, and K. H. Ploog, J. Appl. Phys. 90, 2405 (2001). [82] S. Tomic, E. P. OReilly P. J. Klar, H. Gr€uning, W. Heimbrodt, W. M. Chen, and I. A. Buyanova, Phys. Rev. B 69, 245305 (2004). [83] R. Kudrawiec, M. Motyka, M. Gladysiewicz, J. Misiewicz, J. A. Gupta, and G. C. Aers, Solid State Commun. 138, 365 (2006). [84] T. Kitatani, M. Kondow, T. Kikawa, Y. Yazawa, M. Okai, and K. Uomi, Jpn. J. Appl. Phys. 38, 5003 (1999).

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

303

[85] M. Hetterich, M. D. Dawson, A. Y. Egorov, D. Bernklau, and H. Riechert, Appl. Phys. Lett. 76, 1030 (2000). [86] G. Dumitras, and H. Riechert, J. Appl. Phys. 94, 3955 (2003). [87] J. C. Harmand, A. Caliman, E. V. K. Rao, L. Largeau, J. Ramos, R. Teissier, L. Travers, G. Ungaro, B. Theys, and I. F. L. Dias, Semicond. Sci. Technol. 17, 778 (2002). [88] F. Bousbih, S. B. Bouzid, R. Chtourou, F. F. Charfi, J. C. Harmand, and G. Ungaro, Mater. Sci. Eng. C 21, 251 (2002). [89] S. A. Lourenco, I. F. L. Dias, L. C. Poc as, J. L. Duarte, J. B. B. de Oliveira, and J. C. Harmand, J. Appl. Phys. 93, 4475 (2003). [90] R. Kudrawiec, K. Ryczko, J. Misiewicz, H. B. Yuen, S. R. Bank, M. A. Wistey, H. P. Bae, and J. S. Harris, Jr., Appl. Phys. Lett. 86, 141908 (2005). [91] G. V. Rao, F. S€auberlich, and A. Klein, Appl. Phys. Lett. 87, 032101 (2005). [92] J -J. Chen, F. Ren, Y. Li, D. P. Norton, S. J., Pearton, A. Osinsky, J. W. Dong, P. P. Chow, and J. F. Weaver, Appl. Phys. Lett. 87, 192106 (2005). [93] T. Yokogawa, T. Ishikawa, J. L. Merz, and T. Taguchi, J. Appl. Phys. 75, 2189 (1994). [94] M. Kim, C. S. Kim, S. Lee, J. K. Furdyna, and M. Dobrowolska, J. Cryst. Growth 214/215, 325 (2000). [95] M. W€ort, E. Griebl, T. Reisinger, R. Flierl, B. Haserer, T. Semmler, T. Frey, W. Gebhardt, Phys. Status Solidi B 202, 805 (1997). [96] P. M. Young, E. Runge, M. Ziegler, and H. Ehrenreich, Phys. Rev. B 49, 7424 (1994). [97] F. Liaci, P. Bigenwald, O. Briot, B. Gil, N. Briot, T. Cloitre, and R. L. Aulombard, Phys. Rev. B 51, 4699 (1995). [98] V. Pellegrini, A. Tredicucci, F. Beltram, L. Vanzetti, M. Lazzarino, and A. Franciosi, J. Appl. Phys. 79, 929 (1996). [99] C. Guenaud, E. Deleporte, A. Filoramo, P. Lelong, C. Delalande, C. Morhain, E. Tournie, and J. P. Faurie, J. Appl. Phys. 87, 1863 (2000). [100] V. I. Kozlovsky, Y. G. Sadofyev, and V. G. Litvinov, Nanotechnol. 11, 241 (2000). [101] M. W. Wang, J. F. Swenberg, M. C. Phillips, E. T. Yu, J. O. McCaldin, R. W. Grant, and T. C. McGill, Appl. Phys. Lett. 64, 3455 (1994). [102] H. Mariette, F. Dalbo N. Magnea, G. Lentz, and H. Tuffigo, Phys. Rev. B 38, 12443 (1988). [103] J. Allegre, J. Calatayud, B. Gil, H. Mathieu, H. Tuffigo, G. Lentz, N. Magnea, and H. Mariette, Phys. Rev. B 41, 8195 (1990). [104] E. Deleporte, J. M. Berroir, C. Delalande, N. Magnea, H. Mariette, J. Allegre, and J. Calatayud, Phys. Rev. B 45, 6305 (1992). [105] J. Calatayud, J. Allegre, H. Mathieu, N. Magnea, and H. Mariette, Phys. Rev. B 47, 9684 (1993). [106] V. I. Kozlovsky, Y. G. Sadofyev, and V. G. LItvinov, J. Cryst. Growth 214/215, 983 (2000). [107] von Truchseb M. V. Latussek, F. Goschenhofer, C. R. Becker, G. Landwehr, E. Batke, R. Sizmann, and P. Helgesen, Phys. Rev. B 51, 17618 (1995). [108] A. Qteish, and R. J. Needs, J. Phys.: Condens. Matter 3, 617 (1991). [109] P. M. Young, and E. Ehrenreich, Phys. Rev. B 43, 12057 (1991). [110] R. Sizmann, P. Helgesen, T. Colin, T. Skauli, and S. Lfvold, Appl. Phys. Lett. 64, 881 (1994). [111] Z. Yang, Z. Yu, Y. Lansari, S. Hwang, J. W. Cook, Jr., and J. F. Schetzina, Phys. Rev. B 49, 8096 (1994). [112] von Truchseb M. V. Latussek, C. R. Becker, and E. Batke, J. Cryst. Growth 159, 1128 (1996). [113] D. Eich, K. Ortner, U. Groh, Z. H. Chen, C. R. Becker, G. Landwehr, R. Fink, and E. Umbach, Phys. Status Solidi A 173, 261 (1999). [114] C. R. Becker, V. Latussek, Pfeuffer-Jeschke A. G. Landwehr, and L. W. Molenkamp, Phys. Rev. B 62, 10353 (2000). [115] K. Shahzad, D. J. Olego, C. G. Van de Walle, Phys. Rev. B 38, 1417 (1988). [116] M. Lomascolo, G. H. Li, K. Syassen, R. Cingolani, and I. Suemune, Phys. Rev. B 50, 14635 (1994). [117] S. Li, and J. B. Khurgin, Appl. Phys. Lett. 60, 1969 (1992).

304 [118] [119] [120] [121] [122] [123] [124] [125] [126] [127] [128] [129] [130] [131] [132] [133] [134] [135] [136] [137] [138] [139] [140] [141] [142] [143] [144] [145] [146] [147] [148] [149] [150] [151] [152] [153] [154]

PROPERTIES OF SEMICONDUCTOR ALLOYS S. Li, and J. B. Khurgin, Appl. Phys. Lett. 61, 1694 (1992). E. Pelucchi, S. Rubini, B. Bonanni, A. Franciosi, and M. Peressi, Appl. Phys. Lett. 78, 1574 (2001). Y. Wu, K. Ichino, Y. Kawakami, S. Fuijita, and S. Fujita, Jpn. J. Appl. Phys. 31, 1737 (1992). K. Kondo, H. Okuyama, and A. Ishibashi, Appl. Phys. Lett. 64, 3434 (1994). J. Suda, Y. Kawakami, S. Fujita, and S. Fujita, Jpn. J. Appl. Phys. 33, L986 (1994). T. Miyajima, F. P. Logue, J. F. Donegan, J. Hegarty, H. Okuyama, A. Ishibashi, and Y. Mori, Appl. Phys. Lett. 66, 180 (1995). K. Shahzad, J. Petruzzello, J. M. Gaines, and C. Ponzoni, Appl. Phys. Lett. 67, 659 (1995). H. Hamadeh, M. L€unenb€urger, H. Kalisch, and M. Heuken, J. Cryst. Growth 184/185, 867 (1998). H. P. Wagner, M. K€uhnelt, H. Wenisch, and D. Hommel, Phys. Rev. B 63, 235319 (2001). P. F. Baude, M. A. Haase, G. M. Haugen, K. K. Law, T. J. Miller, K. Smekalin, J. Phillips, and P. Bhattacharya, Appl. Phys. Lett. 68, 3591 (1996). K. Godo, H. Makino, M. W. Cho, J. H. Chang, S. K. Hong, T. Yao, M. Y. Shen, and T. Goto, J. Appl. Phys. 91, 5811 (2002). M. Mun~oz, H. Lu, X. Zhou, M. C. Tamargo, and F. H. Pollak, Appl. Phys. Lett. 83, 1995 (2003). Aubry-Fortuna V. M. Barthula, G. Trembiay, F. Meyer, P. Warren, and K. Lyutovitch, J. Appl. Phys. 89, 5533, (2001), and references cited therein. M. R. H. Khan, H. Nakayama, T. Detschprohm, K. Hiramatsu, and N. Sawaki, Jpn. J. Appl. Phys. 34, 6375 (1995). S. Arulkumaran, T. Egawa, G-Y. Zhao, H. Isikawa, T. Jimbo, and M. Umeno, Jpn. J. Appl. Phys. 39, L351 (2000). D. Qiao, L. S. Yu, S. S. Lau, J. M. Redwing, J. Y. Lin, and H. X. Jiang, J. Appl. Phys. 87, 801 (2000). E. D. Readinger, B. P. Luther, S. E. Mohney, and E. L. Piner, J. Appl. Phys. 89, 7983 (2001). Y. Liu, M. Z. Kauser, P. P. Ruden, Z. Hassan, Y. C. Lee, S. S. Ng, and F. K. Yam, Appl. Phys. Lett. 88, 022109 (2006). A. P. Zhang, G. Dang, F. Ren, J. Han, A. Y. Polyakov, N. B. Smimov, A. V. Govorkov, J. M. Redwing, X. A. Cao, and S. J. Pearton, Appl. Phys. Lett. 76, 1767 (2000). A. Nanda, M. J. Hafich, T. J. Vogt, L. M. Woods, G. A. Patrizi, and G. Y. Robinson, Appl. Phys. Lett. 61, 81 (1992). E. Y. Chang, Y.-L. Lai, K.-C. Lin, and C.-Y. Chang, J. Appl. Phys. 74, 5622 (1993). S. D. Kwon, H. K. Kwon, B. -D. Choe, H. Lim, and J. Y. Lee, J. Appl. Phys. 78, 2482 (1995). J. O. McCaldin, T. C. McGill, and C. A. Mead, J. Vac. Sci. Technol. 13, 802 (1976). Y. Zhu, Y. Ishimaru, N. Takahashi, and M. Shimizu, J. Appl. Phys. 80, 1617 (1996). J. Tersoff, Phys. Rev. B 32, 6968 (1985). L. P. Sadwick, C. W. Kim, K. L. Tan, and D. C. Streit, IEEE Electron Dev Lett. 12, 626 (1991). F. Gueissaz, M. Gailhanou, R. Houdre, and M. Ilegems, Appl. Phys. Lett. 60, 1099 (1992). J.-I. Chyi, J.-L. Shieh, R.-J. Lin, J.-W. Pan, and R.-M. Lin, J. Appl. Phys. 77, 1813 (1995). S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. K. Kajiyama, Y. Mizushima, and S. Sakata, Appl. Phys. Lett. 23, 458 (1973). P. Kordos, M. Marso, R. Meyer, and H. L€uth, J. Appl. Phys. 72, 2347 (1992). C. Marinelli, L. Sorba, M. Lazzarino, D. Kumar, E. Pelucchi, B. H. M€ uller, D. Orani, S. Rubini, A. Franciosi, S. D. Franceschi, and F. Beltram, J. Vac. Sci. Techonol. B 18, 2119 (2000). R. Chin, R. A. Milano, and H. D. Law, Electron. Lett. 16, 627 (1980). W. J. Keeler, A. P. Roth, and E. Fortin, Can. J. Phys. 58, 63 (1980). S. Loualiche, A. L. Corre, S. Salaun, J. Caulet, B. Lambert, M. Gauneau, D. Lecrosnier, and B. Deveaud, Appl. Phys. Lett. 59, 423 (1991). J. H. Zhao, P. F. Tang, and J. Jeong, Solid-State Electron. 35, 21 (1992). J.-K. Lee, Y.-H. Cho, B.-D. Choe, K. S. Kim, H. I. Jeon, H. Lim, and M. Razeghi, Appl. Phys. Lett. 71, 912 (1997).

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT [155] [156] [157] [158] [159] [160] [161] [162] [163] [164] [165] [166] [167] [168] [169]

305

T. Sugino, and T. Kousaka, Electron. Lett. 34, 595 (1998). D. V. Morgan, J. Frey, and W. J. Devlin, J. Electrochem. Soc. 127, 1202 (1980). P. K. Bhattacharya, and M. D. Yeaman, Solid-State Electron. 24, 297 (1981). J. S. Escher, L. W. James, R. Sankaran, G. A. Antypas, R. L. Moon, and R. L. Bell, J. Vac. Sci. Technol. 13, 874 (1976). A. Y. Polyakov, M. Stam, A. G. Milnes, A. E. Bochkarev, and S. J. Pearton, J. Appl. Phys. 71, 4411 (1992). A. Y. Polyakov, A. G. Milnes, L. V. Druzhinina, and I. V. Tunitskaya, Solid-State Electron. 36, 1371 (1993). Y. Liu, H. Jiang, T. Egawa, B. Zhang, and H. Ishikawa, J. Appl. Phys. 99, 123702 (2006). Y. C. Wang, J. M. Kuo, F. Ren, J. R. Lothian, and W. E. Mayo, Solid-State Electron. 42, 1045 (1998). C. Schramm, H. G. Bach, H. K€unzel, and J. P. Praseuth, J. Electrochem. Soc. 138, 2808 (1991). F. E. Akkad, A. Felimban, and F. Sallam, J. Vac. Sci. Technol. A 5, 111 (1987). S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. Q. Li, W. Jie, L. Fu, and G. Zha, Nucl. Instrum. Methods Phys. Res. A 564, 544 (2006). G. Zha, W. Jie, D. Zeng, Y. Xu, W. Zhang, and F. Xu, Surf. Sci. 600, 2629 (2006). X. Cheng, S. Zhu, B. Zhao, Z. He, D. Gao, and J. Fang, Appl. Surf. Sci. 253, 8404 (2007). A. Z. Wang, W. A. Anderson, and M. A. Haase, J. Appl. Phys. 77, 3513 (1995).

10 Optical Properties 10.1 INTRODUCTORY REMARKS 10.1.1 Optical Dispersion Relations The complex dielectric function «ðEÞ ¼ «1 ðEÞ þ i«2 ðEÞ

ð10:1Þ

can be used to describe the optical properties of the medium at all photon energies E ¼ h¯ v [1,2]. The complex refractive index n (E) can also be given by n* ðEÞ ¼ nðEÞ þ ikðEÞ ¼ «ðEÞ1=2 ¼ ½«1 ðEÞ þ i«2 ðEÞ1=2

ð10:2Þ

where n(E) is the ordinary (real) refractive index and k(E) is the extinction coefficient. From Equation (10.2), we obtain «1 ðEÞ ¼ nðEÞ2 kðEÞ2

ð10:3aÞ

«2 ðEÞ ¼ 2nðEÞkðEÞ

ð10:3bÞ

and sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð«1 ðEÞ2 þ «2 ðEÞ2 Þ1=2 þ «1 ðEÞ nðEÞ ¼ 2 sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð«1 ðEÞ2 þ «2 ðEÞ2 Þ1=2 «1 ðEÞ kðEÞ ¼ 2

ð10:4Þ

ð10:5Þ

The absorption coefficient a(E) and normal-incidence reflectivity R(E) can be given by aðEÞ ¼ RðEÞ ¼

4p kðEÞ l

ð10:6Þ

ðnðEÞ1Þ2 þ kðEÞ2 ðnðEÞ þ 1Þ2 þ kðEÞ2

where l is the wavelength of light in vacuum. Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

ð10:7Þ

308

PROPERTIES OF SEMICONDUCTOR ALLOYS

10.1.2 Static and High-frequency Dielectric Constants No detailed experimental data on the static and high-frequency dielectric constants, «s and «¥, of semiconductor alloys have been reported. The simplest linear interpolation scheme for an AxB1xC alloy is «ðxÞ ¼ x«AC þ ð1xÞ«BC

ð10:8Þ

Based on the Clausius–Mossotti relationship, we can also obtain «ðxÞ1 «AC 1 «BC 1 ¼x þ ð1xÞ «ðxÞ þ 2 «AC þ 2 «BC þ 2

ð10:9Þ

It has already been shown that Equations (10.8) and (10.9) give nearly the same results [2]. Readers will find the «s and «¥ values for some non-alloyed group-IV, III–V and II–VI semiconductors in Tables 10.2 and 10.3 of Adachi [1].

10.2 GROUP-IV SEMICONDUCTOR ALLOY 10.2.1 Binary Alloy (a) CSi The n(E) dispersion in 3C-SiC, together with that for diamond and Si, in the region below the fundamental absorption edge is shown in Figure 10.1(a). The experimental data are taken

Figure 10.1 (a) n(E) spectrum for 3C-SiC, together with those for diamond (C) and Si in the region below the fundamental absorption edge at 300 K. The experimental data are taken from Adachi [3]. (b) «(E) spectra for CxSi1x at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Optical characterization of Si1-xCx/Si (0 x 0.014) semiconductor alloys by H. Lee et al., 34, L1340. Copyright (1995), Institute of Pure and Applied Physics]

OPTICAL PROPERTIES

309

from Adachi [3]. Principally, the diamond-type crystals show no reststrahlen structure. Since 3C-SiC has the zinc-blende structure, the reststrahlen peak can be clearly seen in Figure 10.1(a) at E 0.1 eV. The optical properties of CxSi1x (x 0.014) in the IR–UV region have been studied using SE [4,5]. We reproduce in Figure 10.1(b) the «(E) spectra obtained by Lee et al. [5]. We can see that increasing the C concentration decreases the E1 (3.4 eV) and E2 CP strengths (4.3 eV), as has also been observed by Kissinger et al. [4]. (b) CGe The optical properties of CxGe1x with low C concentrations have been studied in the reststrahlen [6] and interband transition regions [6–8]. The optical absorption in the fundamental absorption edge is shifted toward the higher-energy side with increasing x [6,7]. The SE «(E) spectra measured by Krishnamurthy et al. [8] showed that increasing the C concentration decreases the E1=(E1 þ D1) (2.4 eV) and E2 CP strengths (4.2 eV), in a similar manner to that observed in CxSi1x. (c) SiGe The optical properties of relaxed SixGe1x alloy have been studied by many authors [3]. The a(E) spectra in the reststrahlen region of SixGe1x are rather complex due to a number of single- and multiple-phonon bands. The absorption coefficient is weak for the whole composition range, with a peak value of 30 cm1. Figure 10.2 shows, as an example, the reststrahlen absorption spectra for SixGe1x measured by Braunstein [9]. The samples used were selected

Figure 10.2 Far-IR absorption spectra for SixGe1x at 300 K. [Reprinted with permission from R. Braunstein, Phys. Rev. 130, 879–887 (1963). Copyright (1963) American Physical Society]

310

PROPERTIES OF SEMICONDUCTOR ALLOYS

ε2

40 30

8

(a)

x=0 0.11 0.20 0.28 0.48 0.65 0.85 1.00

4 2

SixGe1-x

0 8

(b)

(d)

6

20

4 2

10 0 1

(c)

6 n

50 40 30 20 10 0 -10 -20 50

k

ε1

for homogeneity of composition and low free-carrier concentration. Nevertheless, most of the spectra for 0.22 x 0.81 showed strong background absorption due to free carriers. Bulk single crystals were used in the x from 0 to 0.2 and from 0.9 to 1.0; the intermediate compositions were coarse polycrystals. For several at% Si in Ge or vice versa, the general features of the spectra are similar to the lattice absorption spectra of the dominant constituent, except for slight changes in the positions and shapes of the bands. Aside from the Ge- and Si-like bands present in the alloy, new bands starting at 214 and 508 cm1 are formed at the Ge and Si ends of the alloy, respectively. Both of these bands grow in intensity and shift slightly with position as the Ge and Si content are increased. Braunstein [10] studied the free-hole absorption in p-SixGe1x of various compositions. He observed the intervalence-band absorption and determined some of the VB parameters of this alloy system. The optical absorption in the fundamental absorption edge of SixGe1x has been measured by Braunstein et al. [11]. The optical constants in the IR–UV region of SixGe1x have also been determined by several authors. The «(E) and n (E) spectra for SixGe1x are shown in Figure 10.3. The experimental data are taken from Adachi [3]. The temperature dependence of the optical constants for SixGe1x has also been investigated using SE [3].

2

3 4 E (eV)

5

6

0 1

2

3 4 E (eV)

5

6

Figure 10.3 Optical constants in the IR–UV region of SixGe1x at 300 K. The experimental data are taken from Adachi [3]

The «(E) spectra for strained and relaxed SixGe1x alloys have been determined using SE [12] and it was found that the built-in strain caused a modification of the spectra in the E1 CP region. Ordering in some group-IV semiconductor alloys has also been investigated and in comparison with disordered alloys no large changes in the optical response were found [13]. (d) GeSn The optical properties of GexSn1x (x < 0.2) have been studied using optical absorption [14–16] and SE [17]. The onsets of the direct/indirect optical transitions can be clearly observed in each a(E) spectrum. However, it is difficult to determine which of the onsets is due to the direct (E0) or indirect transitions (EgL) (Figure 6.10(a)). The experimental «(E) spectra for GexSn1x [17] revealed that increasing Sn concentration decreases the E1/(E1 þ D1) (2.2 eV) and E2 CP strengths (4.2 eV). For example, the «2

OPTICAL PROPERTIES

311

strength at the E2 peak decreased from «2(E2)31 (x ¼ 1.0) to 23 (x ¼ 0.82). The CP energies were also found to show strong nonlinearity with respect to x (Figure 6.10(b)).

10.2.2 Ternary Alloy The optical properties of CxSiyGe1xy have been studied by IR absorbance in the phonon absorption region [18], by optical absorption in the fundamental absorption edge [19] and by SE in the IR–UV region [20–22]. The IR absorption spectra [18] showed that the threefold-degenerate localized phonon mode of C defects in Si splits into a number of phonon modes. The a(E) spectrum in the fundamental absorption edge revealed a clear sub-gap absorption tail in an alloy of C0.01Si0.11Ge0.88 with C primarily interstitial, not substitutional [19]. The SE «(E) spectra for CxSiyGe1xy [22] suggested that the CP strengths are reduced slightly and that the absorption at energies E 3 eV is increased with increasing x. The essentially same results have also been obtained by other authors [20,21]. Aella et al. [23] carried out SE measurements on SixGeySn1xy (x 0.25, 1 x y 0.11) and determined the composition dependence of E2 from the spectral derivative analysis.

10.3 III–V SEMICONDUCTOR TERNARY ALLOY 10.3.1 (III, III)–N Alloy (a) c-(III,III)–N alloy The optical constants of c-AlN, c-GaN and c-AlxGa1xN have been determined using SE [24]. We reproduce these results in Figure 10.4. The samples used were grown on GaAs(100) or 3C-SiC(100) by MBE. The n(E) data for c-GaN measured by K€ohler et al. [25] are also shown

Figure 10.4 (a) n(E) and (b) k(E) spectra for c-AlxGa1xN at 300 K. [Reprinted with permission from Jpn. J. Appl. Phy., Optical constants of Cubic GaN, AlN, and AlGaN Alloys by T. Suzuki et al., 39, L497. Copyright (2000), Institute of Pure and Applied Physics]

312

PROPERTIES OF SEMICONDUCTOR ALLOYS

by the solid circles. The refractive indices at l ¼ 400 nm in Figure 10.4 can be written as a function of x as nðxÞ ¼ 2:610 0:880x þ 0:364x2

ð10:10Þ

The n values in c-AlxGa1xN with lower x contents are somewhat larger than those in w-AlxGa1xN, while those with higher x contents are almost equal to the w-AlxGa1xN values. IR reflectivity in c-GaxIn1xN samples (0.769 x 1.000) grown on 3C-SiC/Si(100) by MBE has been measured in the wavenumber range between 450 and 1200 cm1 [26]. SE has also been used to determine the optical constants in the IR–UV region of c-GaxIn1xN (x ¼ 0.93–1.00) grown on GaAs(100) by MBE [27]. A parametric dielectric-function model is used to analyze the experimental SE data. (b) w-AlGaN The «(E) spectra in the IR region of w-AlxGa1xN have been measured by several authors [3,28,29]. These authors demonstrated the sensitivity afforded by IR measurements in determining the optical phonon frequencies. The n(E) dispersion in the transparent region of w-AlxGa1xN has been measured by a number of authors [30–35]. Several authors obtained not only the ordinary-ray n(E) dispersion (no, c?E) but also extraordinary-ray dispersion (ne, c||E) [31,34]. We show in Figure 10.5 the no(E) and ne(E) dispersions in w-AlxGa1xN (0 x 1.0) determined using a prism coupling waveguide technique [31]. The data clearly show the natural birefringence, i.e. Dn ¼ ne no 6¼ 0; its sign is positive for all samples and all wavelengths investigated. The temperature dependence of the n(E) dispersion has also been studied by several authors [30,35]. The absolute a(E) values have been determined for w-AlxGa1xN grown on (0001)-sapphire substrates [36,37]. The a(E) spectra measured by Omnes et al. [36] showed a sharp transition for E close to the excitonic gaps (0 x 0.35); however, the saturated a(E) values above the excitonic peaks (a 2 104 cm1) were about an order of magnitude smaller than those reported by Angerer et al. [37] (0 x 1.0). High-quality w-GaN gave a saturated a value of (1 2) 105 cm1 [3].

Figure 10.5 (a) Ordinary-ray (no) and (b) extraordinary-ray refractive indices (ne) for w-AlxGa1xN at € ur, H. O. Everitt, F. Yun, and H. Morkoç, € Ozg€ 300 K. [Reprinted with permission from G. Webb-Wood, U. Phys. Status Solidi A 188, 793 (2001), Copyright (2001) Wiley–VCH]

OPTICAL PROPERTIES 15

(a)

10

x=0

10

0.11

5

5 0.23

ε2

ε1

0 -5 0.29 0.45 0.53

-10 -15

0

2

E1

E2

E3

0 -5 -10 -15

w-AlxGa1-xN

-20

(b) E0

313

4 6 E (eV)

-20 8

10

2

4

6 E (eV)

8

10

Figure 10.6 «(E) spectra for w-AlxGa1xN at 300 K. Successive spectra are vertically shifted by 4.4, 9.2, 11.6, 18.0 and 21.2, respectively. [Reprinted with permission from C. Buchheim et al., Phys. Status Solidi B 242, 2610 (2005), Copyright (2005) Wiley–VCH]

The SE «(E) spectra for w-AlxGa1xN have been measured by many authors (see e.g. [33,35,38–40]). Figure 10.6 shows the «(E) spectra obtained by Buchheim et al. [40] for samples at x ¼ 00.53. The four CPs (E0 E3) can be clearly seen in the lower x samples. As expected, these CPs undergo a continuous shift to higher energies with increasing x. However, the E3 CP shows a different behavior: it decreases with increasing x to overlap with E2 at high x contents. The origin of such an unusual shift is unclear at present. The «(E)-related optical constants have been interpreted by a simplified interband-transition model, known as the MDF [2,41]. (c) w-AlInN The optical photon behaviors in w-AlxIn1xN with the limited composition of 0.12 x 0.21 have been investigated using IR ellipsometry [42]. The n(E) dispersion in polycrystalline w-AlxIn1xN films has been determined by measuring reflectivity spectra [45]. The modeled n(E) dispersion has also been reported by Laws et al. [43]. The optical absorption spectra a(E) have been measured to determine the fundamental absorption edge in w-AlxIn1xN [44,45]. The SE «(E) spectra for w-AlxIn1xN have been measured by Goldhahn et al. [46]. These results are reproduced in Figure 10.7. The samples used were grown on (0001)-sapphire substrates. The data presented in Figure 10.7 correspond to those for the ordinary ray. The five CPs (E0 E4) can be clearly seen in the «(E) spectra. The unknown peak (A) has also been found in the lower-energy side of the E1 peak. (d) w-GaInN The reflectivity spectra R(E) in the reststrahlen region of w-GaxIn1xN have been measured by Osamura et al. [47]. The samples were polycrystallites grown by electron-beam plasma deposition. The refractive index and natural birefringence in w-GaxIn1xN (0.934 x 0.964) have been determined by a prism coupling method in conjunction with multilayer optical waveguide analysis [48] and found to show positive birefringence (Dn ¼ ne no > 0). Laws et al. [43] obtained the modeled n(E) dispersion curves with x from 0.75 to 0.95. The optical absorption spectra a(E) have also been determined by several authors [49–51].

314

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.7 «(E) spectra for w-AlxIn1xN at 300 K. Successive spectra are vertically shifted by 2.7, 5.1 and 8.7, respectively. [Reprinted with permission from R. Goldhahn et al., Phys. Status Solidi A 203, 42 (2006), Copyright (2006) Wiley–VCH]

The «(E) spectra in the visible–UV region of w-GaxIn1xN have been measured by SE [52,53] and electron energy-loss spectroscopy [54]. The SE «(E) spectra exhibited a clear maximum at the fundamental absorption edge, which allowed the determination of the Ga content x [52]. The «1(E) data in the transparent region have also been analyzed using the Sellmeier-type dispersion model [53].

10.3.2 (III, III)–P Alloy (a) AlGaP AlxGa1xP is one of the least studied III–V ternaries. The IR reflectivity has been measured [55]. The low-temperature a(E) spectra in the fundamental absorption edge of AlxGa1xP (0 x 1.0) have also been determined [56]. The n(E) values at several wavelengths for AlxGa1xP (0 x 0.3) have been measured using a phase diffraction grating method [57]. The «(E) spectra in the visible–UV region of AlxIGa1xP have been measured using SE [58,59]. The «(E) spectra obtained by Choi et al. [59] have been reproduced in Figure 10.8. The samples were grown on GaP(100) by gas-source MBE. The interference oscillations can be seen in the transparent region of the alloys. The energy at which the oscillations disappear provides an estimate of E0. The CPs, such as E0, E1 and E2, can be clearly identified in these spectra. (b) AlInP AlxIn1xP with x 0.5 can be epitaxially grown on GaAs substrate. The optical properties of AlxIn1xP are not well known, except for Al0.5In0.5P. Data on the optical constants of Al0.5In0.5P can be found as the endpoint material of the AlxGayIn1xyP/GaAs quaternary.

OPTICAL PROPERTIES

315

Figure 10.8 «(E) spectra for AlxGa1xP at 300 K. Successive spectra are offset in multiples of 10 for clarity. [Reprinted with permission from S. G. Choi et al., J. Appl. Phys. 87, 1287–1290 (2000). Copyright (2000), American Institute of Physics]

(c) GaInP The IR reflectivity in GaxIn1xP has been measured in the spectral ranges of 260–500 [60] and 220–500 cm1 [61]. Brillouin scattering has been used to determine the complex refractive indices n (E) in the region below the fundamental absorption edge of Ga0.52In0.48P latticematched to GaAs [62]. The optical absorption and hydrostatic-pressure effect at the fundamental absorption edge of GaxIn1xP (0.36 x 0.5) have also been measured by Go~ni et al. [63]. A crossover from direct to indirect fundamental gap is found to occur at p ¼ 5.0 (x ¼ 0.36) and 2.7 GPa (x ¼ 0.5) at 300 K. The optical properties of GaxIn1xP (0.494 x 0.584) grown on GaAs have been investigated using SE [64]. The optical functions of Ga0.52In0.48P lattice-matched to GaAs have also been determined using SE [65,66]. The «(E) and n (E) spectra for Ga0.52In0.48P determined by SE as an endpoint material of the AlxGayIn1xyP/GaAs quaternary [3] are shown in Figure 10.9. The effects of ordering on the optical properties of GaInP2 alloy have

25 15

ε

10 5

5

ε2

0

Ga0.52In0.48P

n

3 2 1

-5 -10

(b)

4

ε1

n, k

20

6

(a)

0 1 2 3 4 5 6 E (eV)

k

0 0 1 2 3 4 5 6 E (eV)

Figure 10.9 Optical constants in the IR–UV region of Ga0.52In0.48P/GaAs at 300 K. The experimental data are taken from Adachi [3]

316

PROPERTIES OF SEMICONDUCTOR ALLOYS

also been investigated using SE [67] and found to be relatively weak, yet significant near the fundamental absorption edge and for the higher-lying CPs.

10.3.3 (III, III)–As Alloy (a) AlGaAs The «(E) and n (E) spectra in the reststrahlen region of AlxGa1xAs (0 x 1.0) [3] have been plotted in Figure 10.10. The experimental data are taken from Adachi [3]. The two phonon bands, GaAs-like and AlAs-like, are clear and distinct in Figure 10.10. No additional structure was found in the frequency range 50–700 cm1 [3]. (a) AlAs-like

160 120 80 40 0 200

n

x 0 0.18 0.36 0.54 1.00

(b) k

ε2

ε1

160 120 GaAs-like 80 40 0 -40 -80 -120 240 200

250 300 350 Frequency (cm -1 )

400

16 14 12 10 8 6 4 2 0 16 14 12 10 8 6 4 2 0 200

(c)

AlxGa1-xAs

250 300 350 Frequency (cm -1 )

(d)

400

Figure 10.10 Optical constants in the reststrahlen region of AlxGa1xAs at 300 K. The experimental data are taken from Adachi [3]

The n(E) dispersion in the transparent region of AlxGa1xAs is shown in Figure 10.11. These curves are obtained from a method for calculating n(E) dispersion below E0 [3,68]. The composition dependence of the strength parameters is expressed as continuous functions of x. This insures that the n(E) dispersion in both optional composition x and photon energy E can be calculated, as demonstrated in Figure 10.11. Aspnes et al. [69] reported the room-temperature optical constants in the near-IR–UV region of AlxGa1xAs of target compositions x ¼ 0–0.80 in steps of 0.10 at energies between 1.5 and 6.0 eV determined by SE. The actual compositions were not different from the target compositions by more than 0.02. The accuracy of the pseudodielectric function at selected wavelengths in the technologically relevant composition range of x ¼ 0–0.5 was less than 2% of its peak value. These results are plotted in Figure 10.12. The optical properties in the far-IR–UV region of GaAs, AlAs and AlxGa1xAs published up until 1992 have been reviewed by Adachi [70]. There have been several publications since 1993. They concern a(E) in the fundamental absorption edge [71], n(E) in the terahertzE0 (Eg) region [72–77] and SE «(E) in the near-IR–UV region [78,79]. (b) AlInAs The absorption coefficients a(E) and refractive indices n(E) of AlxIn1xAs, including Al0.48In0.52As/InP, have been measured by several authors [80–84] (see n(E) in Figure 10.31).

OPTICAL PROPERTIES

317

Figure 10.11 n(E) spectra for AlxGa1xAs with increments in x of 0.1 at 300 K. [Reprinted with permission from S. Adachi, J. Appl. Phys. 58, R1–R29 (1985). Copyright (1985), American Institute of Physics]

(a) n

30 25 20 15 10 5 0 -5 -10 -15 35 30 25 20 15 10 5 0 1

x 0 0.099 0.198 0.315 0.419 0.491 0.590 0.700 0.804 1.000 2

(b) k

ε2

ε1

The optical properties in the interband transition region of AlxIn1xAs have been studied using SE by Rodrıguez and Armelles [58] (0 x 1.0), Dinges et al. [85] (x ¼ 0.48) and Kamlet and Terry [86] (0.305 x 0.635). Figure 10.13(a) shows the «(E) spectra for x ¼ 0.48 obtained by Kamlet and Terry [86]. The n (E) spectra were calculated from these «(E) spectra and are shown in the lower part of Figure 10.13(a). The E1 and E2 peaks can be clearly identified at E3 and 4.6 eV, respectively.

3 4 E (eV)

5

6

6 5 4 3 2 1 0 6 5 4 3 2 1 0 1

(c)

AlxGa1-xAs

(d)

2

3 4 E (eV)

5

6

Figure 10.12 Optical constants in the near-IR–UV region of AlxGa1xAs at 300 K. The experimental data are taken from Adachi [3]

318

PROPERTIES OF SEMICONDUCTOR ALLOYS

(a)

30 20 ε1 10 ε2 0 -10 Ga0.47In0.53As 5 4 n 3 2 k 1 0 6 1 2 3 4 E (eV)

(b)

n, k

n, k

ε

ε

30 20 ε1 10 ε 2 0 -10 Al0.48In0.52As 5 4 n 3 2 k 1 0 1 2 3 4 E (eV)

5

5

6

Figure 10.13 (a) Optical constants in the near-IR–UV region of Al0.48In0.52As/InP at 300 K. The experimental data are taken from Kamlet and Terry [86]. (b) Optical constants in the near-IR–UV region of Ga0.47In0.53As/InP at 300 K. The experimental data are taken from Adachi [3]

(c) GaInAs There have been many reports on the optical properties of GaxIn1xAs. This is especially true for Ga0.47In0.53As lattice-matched to InP [87]. More recently, some authors have carried out reflectivity measurements in the reststrahlen region of GaxIn1xAs to characterize the behavior of the long-wavelength optical phonons in strained epilayers [88–90] and also to elucidate plasma reflection [91]. The n(E) dispersion in GaxIn1xAs (0.53 x 1.00) has been determined from reflectance measurements by Takagi [92]. Note that his extrapolated x ¼ 0.47 value, n 3.43 at E ¼ 1.2 eV, is considerably smaller than that reported by Adachi [3] (n 3.6, see Figure 10.31). The optical properties in the visible–UV region of GaxIn1xAs over the entire composition range (0 x 1.0) have been studied using SE [93,94]. Figure 10.14 shows these results [93]. The peaks in «2 at 2.53 and 4.5 eV correspond to the E1/(E1 þ D1) and E2 CPs,

Figure 10.14 «(E) spectra for GaxIn1xAs at 300 K. Successive spectra are offset by 8 and 7 in (a) and (b), respectively. [Reprinted with permission from T. J. Kim et al., Phys. Rev. B 68, 115323 (2003). Copyright (2003) by the American Physical Society]

OPTICAL PROPERTIES

319

respectively. Several authors also used SE to obtain «(E) spectra for Ga0.47In0.53As/InP. The corresponding «(E)-related spectra are shown in Figure 10.13(b) [3]. A series of strained and relaxed GaxIn1xAs layers on GaAs have also been examined using SE [95–98]. Additional information relating to the critical thickness for pseudomorphic growth of GaxIn1xAs on GaAs has been derived [97].

10.3.4 (III, III)–Sb Alloy (a) AlGaSb

n

The IR optical constants of AlxGa1xSb have been determined in the spectral range of 20–520 cm1 [99–102]. The reststrahlen parameters obtained have been given in tabular form [99,101,102]. The n(E) dispersion in the 0.5–1.3 eV region of AlxGa1xSb (0 x 0.73) has been determined from reflectivity measurements by Ance and Van Mau [103]. These results and those for AlSb and GaSb presented in Adachi [3] are shown in Figure 10.15. The optical absorption spectra a(E) for AlxGa1xSb (x 0.41) have also been measured at 2 K and fitted by taking into account the excitonic effects [104]. 4.3 4.2 4.1 4.0 3.9 3.8 3.7 3.6 3.5 3.4 3.3 3.2 3.1

AlxGa1-xSb x=0 0.10 0.24 0.34 0.42 0.48

1.00

0.73

0.4

0.6

0.8 E (eV)

1.0

1.2

Figure 10.15 n(E) spectra for AlxGa1xSb at 300 K. The experimental data are taken from Adachi [3]

SE has been used to characterize epitaxial AlxGa1xSb layers for different x compositions in the 1.4–6 eV region [102,105,106]. The CP parameters and their composition dependence are determined by performing a standard CP analysis. The «(E) spectra obtained by Choi et al. [106] are reproduced in Figure 10.16. (b) GaInSb The IR reflectivity spectra of GaxIn1xSb have been measured in the range 135–285 cm1 by Brodsky et al. [107] and 100–350 cm1 by Feng et al. [108]. The reststrahlen parameters have been tabulated by Brodsky et al. [107]. The absorption spectra a(E) in the fundamental absorption edge of GaxIn1xSb have also been measured at 300 K [109]. Imai and Adachi [110] have obtained the optical constants in the 1.5–5.4 eV region of GaxIn1xSb using SE at 300 K. The samples were grown by a conventional Bridgman method. The n (E) spectra obtained by Imai and Adachi [110] are shown in Figure 10.17. These authors also determined the x-dependent CP parameters from the MDF analysis.

320

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.16 «(E) spectra for AlxGa1xSb at 300 K. Successive spectra are offset upward from the x ¼ 0.39 spectrum by multiples of 5 for clarity. [Reprinted with permission from S. G. Choi, C. J. Palmstrem, Y. D. Kim, S. L. Cooper, and D. E. Aspnes, J. Appl. Phys. 98, 104108 (2005). Copyright (2005), American Institute of Physics]

10.3.5 Dilute-nitride III–(V, V) Alloy (a) GaNP The IR reflectivity spectra of dilute-nitride GaNxP1x have been measured in the spectral ranges of 300–600 cm1 (0.006 x 0.0285) [111] and 50–4000 cm1 (0 x 0.15) [112]. These spectra led to the determination of the GaN- and GaP-like phonon frequencies. The nature of the fundamental absorption edge of GaNxP1x was elucidated using the a(E) spectra [113–115]. The experimental data obtained by Rudko et al. [113] suggest that the absorption edge of GaNxP1x with x ¼ 0.01–0.03 exhibits a direct band-gap-like behavior. The a(E) spectra obtained by Buyanova et al. [114] have been explained by the BAC model (Section 6.3.5). On the other hand, the low-temperature absorption data obtained by

Figure 10.17 n(E) and k(E) spectra for GaxIn1xSb with increments in x of 0.25 at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Optical constants of In1-xGaxSb ternary alloys: Experiment and modeling by S. Imai and S. Adachi, 32, 3860. Copyright (1993), Institute of Pure and Applied Physics]

OPTICAL PROPERTIES

321

Fluegel et al. [115] indicate that the host CB minimum near X does not plunge downward with increased N doping. These results challenge the validity of the BAC and polymorphous model for GaNxP1x, but corroborate the conclusion that due to the dissimilarity between GaNxP1x and GaNxAs1x, seeking a universal model for the band-gap lowering that applies to both the isoelectronic doping systems is unrealistic. SE has been used to investigate the electronic energy-band structure of GaNxP1x [114,116]. The «2(E) spectra obtained by Leibiger et al. [116] are reproduced in Figure 10.18. The vertical dotted lines mark the CPs, E0, E1, E00, E2 and E10, determined by MDF analysis.

Figure 10.18 «2(E) spectra for dilute-nitride GaNxP1x at 300 K. Successive spectra are offset in multiples of 4 for clarity [Reprinted with permission from G. Leibiger, V. Gottschalch, M. Schubert, G. Benndorf, and R. Schwabe, Phys. Rev. B 65, 245207 (2002). Copyright (2002) by the American Physical Society]

(b) GaNAs The absorption coefficient a(E) in the fundamental absorption edge of GaNxAs1x has been measured by several authors (see e.g. [117–119]). The a(E) spectra recorded by Tisch et al. [119] (0 x 0.05) are shown in Figure 10.19. It can be seen that for all samples a2 depends linearly on E up to 108 cm2. The slope of the linear part of a2 decreases and the Urbach tail increases with increasing N fraction. The decrease in the fundamental absorption edge (E) with increasing x can be clearly seen (see also Figure 6.29(b)). The optical properties of GaNxAs1x have been studied using SE by many authors (see e.g. [120–122]). The «(E) spectra recorded by Leibiger et al. [122] are shown in Figure 10.20. The «(E)-related spectra, «(E) and n (E), were found to agree very well with the MDF approach [120–122]. Note that the fundamental absorption edge (E) observed in Figure 10.20 follows the well-known redshift with increasing x. (c) GaNSb FTIR measurements on GaNxSb1x have been undertaken by Jefferson et al. [123]. The divergence of transitions from the VB to E and E þ has been observed with increasing N incorporation, consistent with the BAC model (Figure 6.29(c)).

322

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.19 a2 versus E plots for dilute-nitride GaNxAs1x at 300 K. [Reprinted with permission from U. Tisch, E. Finkman, and J. Salzman, Appl. Phys. Lett. 81, 463 (2002). Copyright (2002), American Institute of Physics]

(d) InNP Optical absorption measurements were carried out to investigate the N incorporation effect into InP [124]. A band-gap reduction of 0.15 eV was observed with N incorporation of 0.9 at%. (e) InNAs IR reflectivity and Hall-effect measurements have been carried out to determine the x-dependent electron effective mass in InNxAs1x [125] (Figure 7.11). The N-induced reduction of the fundamental absorption edge has also been confirmed in InNxAs1x by plotting a2 versus E [126] (Figure 6.31(b)).

10.3.6 Al–(V, V) Alloy An AlPSb layer lattice-matched to InP was grown by gas-source MBE [127]. Using an ellipsometer, the refractive index of this alloy at l ¼ 1.55 mm was determined to be 3.037.

Figure 10.20 «(E) spectra for dilute-nitride GaNxAs1x at 300 K. Successive spectra are offset upward from the x ¼ 0.10 at% spectrum by multiples of 3 for clarity. [Reprinted with permission from G. Leibiger, and M. Schubert, J. Appl. Phys. 89, 4927 (2001). Copyright (2001), V. Gottschalch, B. Rheinl€ander, J. Sik, American Institute of Physics]

OPTICAL PROPERTIES

323

Saadallah et al. [128] carried out photothermal deflection measurements on an MBE-grown AlAs0.08Sb0.92/GaSb layer and determined the n(E) and a(E) spectra, in addition to the thickness of the layer and its thermal conductivity. The Sellmeier parameters which were determined are: A ¼ 8.82, B ¼ 0.79 and C ¼ 0.589 mm (see Equation (10.71) in Adachi [1]). The fundamental absorption edge of AlAs0.08Sb0.92 was also estimated to be 1.55 eV (Figure 6.32(b)).

10.3.7 Ga–(V, V) Alloy (a) GaPAs The n(E) dispersion in GaPxAs1x has been studied by several authors [129–131]. The n(E) data obtained by Clark and Holonyak [129] and Casey [130] agree closely between 1.2 and 1.75 eV where comparison is possible. The experimental data at 87 and 300 K by Clark and Holonyak [129] were fitted to the first-order Sellmeier equation. This enables us to calculate the n(E) dispersion in a given alloy of composition x and photon energy E. These results are shown in Figure 10.21. The calculated n(E) values are taken from Adachi [3]. The resulting n(E) dispersion is found to decrease with increasing x. 3.6 3.5

n

3.4

x=0

3.3 3.2 GaPxAs1-x

3.1 3.0 0.4

x=1.0

0.8

1.2 1.6 E (eV)

2.0

2.4

Figure 10.21 n(E) dispersion in the transparent region of GaPxAs1x with increments in x of 0.1 at 300 K. The n values are taken from Adachi [3]

Clark and Holonyak [129] investigated the optical absorption spectra in the IR and fundamental absorption edge regions of GaPxAs1x. They observed the free-carrier and interconduction-band absorption in GaAs-rich alloys and donor-related absorption in GaP-rich alloys. The Burstein–Moss shift of the fundamental absorption edge was also observed. The optical absorption in GaPxAs1x (0.29 x 0.43) has also been examined by Nelson et al. [132] who observed distinct free-exciton peaks (n ¼ 1 and 2) at 4.2 K and a peak (n ¼ 1) at T 77 K. The direct-exciton binding energy G for GaPxAs1x obtained by Nelson et al. [132] is plotted in Figure 10.22 as a function of x, together with the corresponding values for GaP and GaAs taken from Adachi [1]. The direct-exciton (E0) and indirect-exciton binding energies (EgX ) for GaP are 13 and 22 meV, respectively (see Table 10.4 in Adachi [1]). The G values for GaPxAs1x in Figure 10.22 are considerably smaller than those obtained from the linear interpolation scheme. Thomson et al. [133] measured the fundamental reflectivity spectra of GaPxAs1x at 80 and 295 K. More recently, Kim et al. [134] reported the «(E) spectra of GaPxAs1x layers grown

324

PROPERTIES OF SEMICONDUCTOR ALLOYS 20 GaPxAs1-x

G (meV)

15 10 5 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 10.22 Direct-exciton binding energy G versus x for GaPxAs1x. The experimental data (solid circles) are taken from Nelson et al. [132]. The open squares show the endpoint binary data taken from Adachi [1]

by VPE on GaAs(100) (x ¼ 0.2 and 0.4) and on GaP(100) (x ¼ 0.7). The measured «(E) spectra revealed distinct structures at energies of the E0, E1, E1 þ D1, E00 and E2 CPs. (b) GaPSb GaPxSb1x lattice-matched to InP was grown by gas-source MBE [127]. Using an ellipsometer, the refractive index of this alloy at l ¼ 1.55 mm was determined to be 3.579. A highly reﬂective distributed Bragg reﬂector was demonstrated using AlPxSb1x/GaPxSb1x, which showed a stop-band width of 206 nm with maximum reflectivity exceeding 99% at l 1.6 mm. (c) GaAsSb The IR reflectivity spectra of GaAsxSb1x have been measured in the 200–320 cm1 range by Lukovsky and Chen et al. [135]. A reflectance band was observed in the x ¼ 0.85 composition, whereas at least two bands were evident in the x ¼ 0.20 and 0.25 samples. In the latter two samples, the structure near 240 cm1 was due to the phonon modes, whereas the structure at lower energies (230 cm1) was due to free-carrier plasma effects. Optical absorption measurements were undertaken on GaAsxSb1x by several authors [136–138]. The measured data were used to determine E0 [136] and its temperature dependence [137,138]. The fundamental reflectivity spectra were measured on evaporated GaAsxSb1x films on glasses and on bulk samples [139]. SE and PR were used to determine the x dependence of some CPs, such as E0, E1 and E2, in epitaxial GaAsxSb1x/GaAs(100) layers (0.44 x 1.00) [140]. More recently, Serries et al. [141] used SE and Raman scattering to investigate pseudomorphically strained GaAsxSb1x layers (0.35 x 0.78) grown on InP(100).

10.3.8 In–(V, V) Alloy (a) InPAs The reflectivity spectra in the reststrahlen region of InPxAs1x have been measured by several authors [142,143]. These studies gave similar results; however, the InP- and InAs-like

OPTICAL PROPERTIES

325

oscillator strengths determined by Lockwood et al. [143] vary considerably from those reported by Kekelidze et al. [142]. The plasma reflection characteristics have also been studied by Charache et al. [91]. The alloy composition dependence of E0 has been determined by plotting a2 versus E [144]. The «(E) spectra have also been obtained for InPxAs1x/InP(100) samples using SE [145]. The x dependence of the E1, E1 þ D1 and E2 CPs have been determined by analyzing the second-derivative spectra of «(E). The «(E) spectra obtained by Choi et al. [145] have been reproduced in Figure 10.23.

Figure 10.23 «(E) spectra for InPxAs1x at 300 K. Successive spectra are offset in multiples of 10 for clarity [Reprinted with permission from S. G. Choi, C. J. Palmstrøm, Y. D. Kim, D. E. Aspnes, H. J. Kim, and Y.-C. Chang, Appl. Phys. Lett. 91, 041917 (2007). Copyright (2007), American Institute of Physics]

(b) InPSb The optical absorption spectra a(E) have been measured to determine the x dependence of E0 for MOCVD-InPxSb1x layers [146] (Figure 6.37(a)). The spectra show long band tails, which extend further into the gap as the Sb concentration is increased. The band tails are considered to be caused by compositional clustering. (c) InAsSb The optical reflectivity in the reststrahlen region of InAsxSb1x has been studied in the 135–285 cm1 range by Lucovsky et al. [135] and in the 50–300 cm1 range by Rowell et al. [147]. Plasma-edge reflectance data obtained by Thomas and Woolley [148] suggested that «¥ for InAsxSb1x can be given by the linear interpolation between the endpoint binary data within experimental accuracy. Optical absorption and transmittance measurements have been carried out to characterize InAsxSb1x layers grown on GaAs [149,150], GaSb [151] and InAs [152]. The data are mainly used to determine E0 in these alloy layers. Note that all these substrates are transparent for light wavelengths at or below the InAsxSb1x gap (0 x 1.00). SE measurements have been undertaken for InAsxSb1x layers grown on InAs(100) [153,154]. The alloy compositions investigated were 0.89 x 0.96 [153] and 0 x 0.06 [154].

326

PROPERTIES OF SEMICONDUCTOR ALLOYS

10.4 III–V SEMICONDUCTOR QUATERNARY ALLOY 10.4.1 Dilute-nitride Quaternary Alloy (a) GaInNP The optical properties of GaxIn1xNyP1y epilayers on GaP(100) have been investigated using SE [155]. The compositions of GaxIn1xNyP1y layers were changed to satisfy the latticematching condition, i.e. x 1y, with 0 y 0.035. The SE-derived spectra, n(E), k(E) and a(E), were presented in graphical form. (b) GaInNAs Far-IR SE has been used to investigate the reststrahlen properties of GaxIn1xNyAs1y (x > 0.87, y < 0.03) [156]. The plasma reflection spectra have also been measured to determine the CB dispersion relationships in GaxIn1xNyAs1y [157]. This study also reported the temperature- and pressure-dependent optical absorption at the fundamental absorption edge of free-standing GaxIn1xNyAs1y layers (0.91 x 1.00, 0 y 0.025) lattice-matched to GaAs. The n(E) dispersion in the transparent region of strained GaxIn1xNyAs1y layers has been measured by several authors [156,158]. The SE-derived n(E) and k(E) spectra were analyzed using the MDF approach [156]. The SE «(E) spectra in the interband transition region of GaxIn1xNyAs1y have also been reported by Skierbiszewski [157]. These results have been reproduced in Figure 10.24. It can be seen that the N incorporation has a large effect on the optical dispersion relationships in the E1/(E1 þ D1) transition region (3 eV).

Figure 10.24 «(E) spectra for dilute-nitride GaxIn1xNyAs1y at 300 K. Successive spectra are offset in multiples of 5 for clarity [Reprinted with permission from C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002), Copyright (2002) Institute of Physics]

10.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs The IR reflectivity spectra in the 200–500 cm1 range of AlxGa1xPyAs1y have been measured by Sen and Lucovsky [159]. The reststrahlen parameters obtained were reported in tabular form. The optical absorption spectra a(E) at the fundamental absorption edge of

OPTICAL PROPERTIES

327

AlxGa1xPyAs1y have also been measured by Kuznetsov et al. [160]. The single-crystalline alloys used were grown on GaP by LPE with several pairs of composition (x, y). (b) AlGaAsSb The IR reflectivity spectra in the range of 75–400 cm1 for AlxGa1xAsySb1y/GaSb have been measured by Mezerreg et al. [161]. The reststrahlen parameters obtained were presented in tabular form. Alibert et al. [162] obtained the n(E) dispersion in LPE-grown AlxGa1xAsySb1y/GaSb layers. The n(E) data were determined from accurate measurement of the p-polarized light reflection as a function of the incident angle. The data in the limit E ! 0 eV (i.e. «¥ values) showed very strong nonlinearity with respect to x [162]. The n(E) data for AlxGa1xAsySb1y/ InP (x ¼ 0.1) have also been determined from reflectance measurements [163]. The n(E) dispersion in AlxGa1xAsySb1y/InP obtained from the MDF calculation [2] is shown in Figure 10.25. The solid circles represent the experimental data taken from Blum et al. [163].

Figure 10.25 n(E) dispersion in the transparent region of AlxGa1xAsySb1y/InP with increments in x of 0.1 at 300 K, together with that for InP. The n(E) curves are calculated from the simplified interbandtransition model [2]. The experimental data by Blum et al. [163] are represented by the solid circles (x ¼ 0.1)

The absorption coefficients for LPE-grown AlxGa1xAsySb1y layers on GaAs with (x, y) ¼ (0, 0.9) and (0.06, 0.9) have been determined at several temperatures between 20 and 300 K [164]. Note that this material system is not a lattice-matched system. (c) GaInPAs The IR reflectivity spectra of GaxIn1xPyAs1y/InP have been measured by several authors [3]. The optical constants in the reststrahlen region can be usually determined by using KramersKr€ onig transformation or from the fit to an oscillator model. However, no detailed reststrahlen parameters have been determined for GaxIn1xPyAs1y/InP. This is because many IR studies were focused on multi-phonon behaviors (Section 4.2).

328

PROPERTIES OF SEMICONDUCTOR ALLOYS

The n(E) measurements in the transparent region were carried out using various techniques [3]. Accurate experimental data relating to the optional composition of GaxIn1xPyAs1y are, however, not yet available. Thus, some type of calculation is necessary. Different approaches have been used to calculate the n(E) dispersion. Our calculated n(E) curves for InxGa1xAsyP1y=InP based on the simplified interband-transition model [2] are presented in Figure 10.26.

Figure 10.26 n(E) dispersion in the transparent region of GaxIn1xPyAs1y/InP with increments in y of 0.1 at 300 K. The n(E) curves are calculated from the simplified interband-transition model [2]

Near-band-edge absorption in GaxIn1xPyAs1y/InP has been studied by many investigators [3]. The spectra depicted the sharp decline of a, common to the direct-band-gap semiconductors. Since the experimental information seemed to be limited to narrow composition and wavelength ranges, Fiedler and Schlachetzki [165] calculated the absorption coefficients for GaxIn1xPyAs1y using the extrapolation scheme. The optical constants in the interband transition region of GaxIn1xPyAs1y/InP have been studied using SE [3]. Kelso et al. [166] reported the room-temperature optical constants for GaxIn1xPyAs1y/InP of target compositions y ¼ 0–1.0 in steps of 0.2 at energies E ¼ 1.5–6.0 eV measured by SE. The samples were grown by LPE with carrier concentrations in the 1016–1017 cm3 range. The complex optical constants, «(E) and n (E), obtained from this study [3,166] are shown in Figure 10.27. The n(E) data in the transparent region (l ¼ 808, 850 and 980 nm) of GaxIn1xPyAs1y/ GaAs have been determined using variable-angle SE [167]. As expected, the n value decreased with increasing E0, i.e. increasing y (Figure 6.44(a)). (d) GaInAsSb The IR reflectivity spectra for GaxIn1xAsySb1y/GaSb epilayers have been measured by Mezerreg et al. [161] and Pickering [168]. The reststrahlen parameters obtained were presented in tabular form [161]. Studies on GaxIn1xAsySb1y/InAs have also been undertaken by Pickering [168]. Bi et al. [169] reported the IR absorption properties of MBE-grown GaxIn1xAsySb1y layers on GaAs and GaSb substrates. They also obtained n(E) curves in the 600–3200 cm1 range

25 20 15 10 5 0 -5 -10 25

5

(a)

4 3 2

y=0 0.18 0.45 0.58 0.76 1.00

1

(b)

(c)

3

15 10

2 1

5 0

Gax In1-x PyAs1-y /InP

0 4

k

ε2

20

329

n

ε1

OPTICAL PROPERTIES

(d) 2

3

4 E (eV)

5

6

0

2

3

4 E (eV)

5

6

Figure 10.27 Optical constants in the near-IR–UV region of GaxIn1xPyAs1y=InP at 300 K. The experimental data are taken from Adachi [3]

with (x, y) ¼ (0.734, 0.109) and (0.753, 0.093). These data agreed well with the theoretical prediction by Adachi [2,170]. From the far-field patterns in a GaxIn1xAsySb1y=AlxGa1xAsy Sb1y=GaSb double-heterostructure laser of lasing wavelength at 2.2 mm, Loural et al. [171] determined the active-layer n value to be 3.78. This value exactly agrees with the theoretical prediction based on the simplified interband-transition model [2,170]. Figure 10.28 shows the n(E) curves with x increments of 0.1 for (a) GaxIn1xAsySb1y/GaSb and (b) GaxIn1xAsySb1y/InAs calculated from the simplified interband-transition model [2,170].

Figure 10.28 n(E) dispersion in the transparent region of (a) GaxIn1xAsySb1y=GaSb and (b) GaxIn1x AsySb1y=InAs with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the simplified interband-transition model [2,170]

330

PROPERTIES OF SEMICONDUCTOR ALLOYS

The high-energy endpoint on each curve in Figure 10.28 corresponds to the n value at the band edge E0. A noticeable feature found in this figure is that these alloy systems show a refractive-index anomaly, i.e. the smaller E0-gap material has a smaller refractive index. Note that almost all III–V and II–VI semiconductor alloys, such as AlxGa1xAs and GaxIn1xPyAs1y, show no such anomalies in refractive-index (Figures 10.11 and 10.26).

10.4.3 (III, III, III)–V Alloy (a) AlGaInP The IR properties of (AlxGa1x)0.53In0.47P/GaAs have been studied by Hofmann et al. using far-IR SE [172]. They suggested that far-IR SE may be used to identify small degrees of longrange ordering in this quaternary. By fitting the SE n(E) data with the first-order Sellmeier equation, Adachi et al. [173] determined a set of the dispersion parameters A, B and C in the transparent region of the (AlxGa1x)0.53In0.47P quaternary that can be written as (C in mm) AðxÞ ¼ 5:38 þ 2:16x

ð10:11aÞ

BðxÞ ¼ 4:013:01x

ð10:11bÞ

CðxÞ2 ¼ 0:184 0:019x þ 0:024x2

ð10:11cÞ

As l ! ¥ in the fist-order Sellmeier equation, we obtain n(l ! ¥)2 ¼ «¥ ¼ A þ B. Figure 10.29 shows the n(E) dispersion with increments in x of 0.1 for (AlxGa1x)0.53 In0.47P/GaAs calculated from the simplified interband-transition model [2]. The solid circles represent the experimental data for x ¼ 0, 0.42 and 1.0 obtained by Tanaka et al. [174].

Figure 10.29 n(E) dispersion in the transparent region of (AlxGa1x)0.53In0.47P/GaAs with increments in x of 0.1 at 300 K, together with that for GaAs. The n(E) curves are calculated from the simplified interband-transition model [2]. The solid circles represent the experimental data for x ¼ 0, 0.42 and 1.0 reported by Tanaka et al. [174]

The optical constants in the interband transition region of (AlxGa1x)0.53In0.47P/GaAs have been measured by SE [3]. Figure 10.30 shows the complex optical constants, «(E) and n (E), taken from

20 15 10 5 0 -5 -10 25

(c)

3

1 4

(b)

3

15 k

ε2

4

2

x 0 0.25 0.50 0.75 1.00

20 10

(AlxGa1-x)0.53In0.47P/GaAs

(d)

2 1

5 0

331

5

(a) n

ε1

OPTICAL PROPERTIES

1

2

3

4

5

6

0

1

2

E (eV)

3

4

5

6

E (eV)

Figure 10.30 «(E)-related spectra in the IR–UV region of (AlxGa1x)0.53In0.47P/GaAs at 300 K. The experimental data are taken from Adachi [3]

Adachi [3]. The two major features seen in Figure 10.30 are due to the E1 and E2 CPs at 3.2–3.7 eV and 4.8 eV, respectively. The E1 structure moves toward higher energy with increasing x, while the E2 structure does not perceptibly do so. The E1 þ D1 structure is not clearly discernible in (AlxGa1x)0.53In0.47P/GaAs. These spectra were fitted by the MDF very well [175,176]. (b) AlGaInAs The n(E) dispersion in the transparent region and in the region a little above the E0 edge of (AlxGa1x)0.48In0.52As has been measured by several authors [3]. Figure 10.31 shows the experimental n(E) data for (AlxGa1x)0.48In0.52As/InP. These data are taken from Adachi [3]. Mondry et al. [82] modeled the experimental n(E) data with the first-order Sellmeier equation. The heavy solid lines in Figure 10.31 represent the endpoint ternary data that they obtained. The fundamental absorption edge in (AlxGa1x)0.48In0.52As/InP has been measured by Masu et al. [177]. The spectra showed a sharp decline in a(E), common to direct-band-gap 3.8 (AlxGa1-x)0.48In0.52As/InP

3.7 3.6

x=0 (GaInAs)

n

3.5 3.4

0.27

3.3 0.49 0.54

3.2 0.75 3.1 0.4

1.00 (AlInAs)

0.6

0.8 1.0 E (eV)

1.2

1.4

Figure 10.31 n(E) dispersion in (AlxGa1x)0.48In0.52As/InP at 300 K. The experimental data are taken from Adachi [3]. The heavy solid lines represent the endpoint ternary data by Mondry et al. [82]

332

PROPERTIES OF SEMICONDUCTOR ALLOYS

semiconductor materials. Using LPE Swarup et al. [178] also measured the absorption spectra of AlxGayIn1xyAs layers grown on the (111)As face of GaAs substrates. The optical constants in the interband transition region of (AlxGa1x)0.48In0.52As/InP have been determined using SE [3]. The refractive indices in the wavelength range 1.0–1.9 mm of (AlxGa1x)0.48In0.52As/InP have also been determined by SE [179]. The n(E) curves with increments in x of 0.1 for (AlxGa1x)0.48In0.52As/InP calculated from the simplified interbandtransition model [2] are shown in Figure 10.32.

Figure 10.32 n(E) dispersion in the transparent region of (AlxGa1x)0.48In0.52As/InP with increments in x of 0.1 at 300 K, together with that for InP. The n(E) curves are calculated from the simplified interband-transition model [2,3]

10.4.4 III–(V, V, V) Alloy A very limited number of reports are available for the optical properties of III–(V, V, V) quaternaries. The IR reflectivity spectra for InPxAsySb1xy layers grown on (111)InAs have been measured by Belov et al. [180]. The optical transmission measurements on LPE-grown InPxAsySb1xy/InAs have also been carried out by Esina et al. [181]. Adachi [3] calculated the n(E) dispersion in AlPxAsySb1xy, GaPxAsySb1xy and InPxAsySb1xy lattice-matched to GaAs, InP or InAs with increments in x of 0.1 using the simplified interband-transition model.

10.5 II–VI SEMICONDUCTOR ALLOY 10.5.1 (II, II)–O Ternary Alloy (a) BeZnO Transmittance measurements on BexZn1xO/sapphire samples have been carried out [182,183]. The measured spectra are used to determine the composition dependence of E0 (Figure 6.54(a)). (b) MgZnO The reststrahlen properties of MgxZn1xO have been investigated using far-IR reflectivity [184] and SE [185]. Variation in the optical phonon modes with x has been determined in the hexagonal and cubic regions [185].

OPTICAL PROPERTIES

333

The n(E) dispersion in w-MgxZn1xO has been determined for x in the hexagonal [186,187] and cubic regions [188,189]. The n values obtained by Teng et al. [187] have been reproduced in Figure 10.33. The thermo-optical coefficient dn/dT for c-MgxZn1xO (0.57 x 1.0) has also been determined by Zhou et al. [190].

Figure 10.33 Ordinary-ray (no) and extraordinary-ray refractive-index spectra (ne) for w-MgxZn1xO at 300 K, together with that for c-MgO. [Reprinted with permission from C. W. Teng et al., Appl. Phys. Lett. 76, 979 (2000). Copyright (2000), American Institute of Physics]

The absorption coefficient a(E) in the fundamental absorption edge of w-MgxZn1xO has been reported [187]. The pressure dependence of a(E) has also been reported [191]. The optical properties in the interband transition region of MgxZn1xO have been investigated using SE [186,192–194] and reflectivity [195]. The SE «(E) spectra for w-MgxZn1xO obtained by Kang et al. [192] have been reproduced in Figure 10.34. The n ¼ 1 excitonic peak can clearly be seen in the «(E) spectra. This is especially true for samples with low x. The higher-lying CPs can also be identified at 7 and 9 eV for x ¼ 0–0.53 [193]. (c) ZnCdO The optical absorption spectra a(E) in the fundamental absorption edge of CdxZn1xO have been measured by several authors [196–199]. The data were used to determine the composition dependence of E0 (Figure 6.54(c)).

10.5.2 (II, II)–S Ternary Alloy (a) MgZnS The optical absorption in w-MgxZn1xS has been measured for 0 x 0.25 [200]. The samples were grown on (0001)-sapphire substrates by PLD. The absorption edge showed blueshift with increasing x (Figure 6.55(a)).

334

PROPERTIES OF SEMICONDUCTOR ALLOYS 12

18 (a)

(b)

16

10 0.21

+9.5

12 0.14

+8.0

10 8

0.11

2

4

x=0

+4.0 0.11 +2.0 0.08

2 0

2.0 2.4 2.8 3.2 3.6 4.0 4.4 4.8 E (eV)

+7.0

0.14

6

+3.0

6 4

8

+5.0 0.08

w-MgxZn1-xO 0.21

ε2

ε1

14

+8.0

x=0 2.0 2.4 2.8 3.2 3.6 4.0 4.4 4.8 E (eV)

Figure 10.34 «(E) spectra for w-MgxZn1xO at 300 K. [Reprinted with permission from Solid State Commun., Spectroscopic ellipsometry study of Zn1–xMgxO thin films deposited on Al2O3(0001) by J. H. Kang, Y. R. Park and K. J. Kim, 115, 127–130. Copyright (2000), Elsevier]

(b) ZnCdS Transmittance and reflectance measurements in the reststrahlen region of w-ZnxCd1xS have been carried out by Lisitsa et al. [201]. The n(E) dispersion in c-ZnxCd1xS has also been studied by reflectivity measurements [202]. These results are reproduced in Figure 10.35. Optical absorption a(E) in the fundamental absorption edge of w-CdxZn1xS has been measured at 77 and 150 K [203]. The samples were grown by a sublimation method. The pressure

Figure 10.35 n(E) dispersion in the transparent region of c-ZnxCd1xS at 300 K. The dashed curves correspond to x ¼ 0.83, 0.91, 0.95 and 0.983 from right to left. [From P. Chen et al., Semicond. Sci. Technol. 13, 1439 (1998), Copyright (1998) Institute of Physics]

OPTICAL PROPERTIES

335

dependence of the fundamental absorption edge has also been measured on chemical-transportgrown w-CdxZn1xS layers up to their respective phase transition [204].

10.5.3 (II, II)–Se Ternary Alloy (a) BeZnSe The n(E) dispersion in c-BexZn1xSe layers grown on GaAs substrates by MBE has been measured using a prism coupler technique [205]. The data were fitted to the Sellmeier dispersion equation. These results are shown in Figure 10.36, together with the n(E) dispersion in ZnSe (x ¼ 0) [3]. 3.0 2.9

n

2.8

c-BexZn1-xSe

2.7

x=0 (ZnSe)

2.6 2.5 2.4 2.3 0.8

1.0

1.2

1.6

2.0 2.4 E (eV)

2.8

3.2

Figure 10.36 n(E) dispersion in the transparent region of c-BexZn1xSe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Peiris et al. [205]. The ZnSe data are taken from Adachi [3]

The optical properties of c-BexZn1xSe have been studied using SE in the spectral ranges 2.5–29 eV [206], 1.5–6.0 eV [207] and 1.255.0 eV [208]. The SE «2(E) spectra for c-BexZn1xSe with 0 x 1.0 and E ¼ 2.59 eV [206] are reproduced in Figure 10.37. The very weak structures due to the Zn 3d transitions were identified in the spectral region above 10 eV. (b) BeCdSe SE was used to obtain the «(E) spectra in the range of 0.756.5 eV for w-BexCd1xSe with x ¼ 0.075 [209,210]. The E0, E1 and E2 CPs were identified at 2, 4 and 6 eV, respectively. The alloys at x 0.1 were also grown, but they exhibited chemical instability. (c) MgZnSe The n(E) dispersion in c-MgxZn1xSe layers grown on GaAs(100) and silica glasses by MBE has been measured by Peiris et al. [211] and Derkowska et al. [212], respectively. Peiris et al. [211] reported the first-order Sellmeier constants as a function of x. The n(E) dispersion calculated using these constants, together with the experimental n(E) data for ZnSe (x ¼ 0) [3] are shown in Figure 10.38. The bold solid line is also obtained from the first-order Sellmeier parameters for ZnSe [213]. The absorption coefficients a(E) in the fundamental absorption edge of MBE-grown c-MgxZn1xSe/GaAs layers (0 x 0.36) have been measured at 2 K by W€orz et al. [214]. These results have been reproduced in Figure 10.39. The E0 and E0 þ D0 excitons can be

336

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.37 «2(E) spectra for c-BexZn1xSe at 300 K. [Reproduced with permission from K. Wilmers et al., J. Electron. Mater. 28, 670–677 (1999), Copyright (1999) Springer Science and Business Media]

clearly detected for x up to 0.28. The difference between the n ¼ 1 (1s) and 2 (2s) excitons yields the Rydberg energy

n

4 Ry* ¼ ðE1s E2s Þ 3 3.0 2.9 2.8 2.7 2.6 2.5 2.4 2.3 2.2 0.5

ð10:12Þ

c-MgxZn1-xSe x = 0 (ZnSe)

0.5

1.0

1.5

2.0 2.5 E (eV)

3.0

Figure 10.38 n(E) dispersion in the transparent region of c-MgxZn1xSe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Peiris et al. [211]. The bold solid line (ZnSe) is also calculated from the first-order Sellmeier parameters reported by Adachi [213]. The ZnSe data are taken from Adachi [3] (solid circles)

OPTICAL PROPERTIES

337

Figure 10.39 a(E) spectra in the fundamental absorption edge of MBE-grown c-MgxZn1xSe/GaAs layers (0 x 0.36) at 2 K. [Reprinted with permission from M. W€ orz et al., Phys. Status Solidi B 202, 805 (1997), Copyright (1997) Wiley–VCH]

which in this case, is equal to the exciton binding energy G. The composition dependence obtained by W€ orz et al. [214] can be written as G ¼ (20 0.2) þ (37.5 7)x meV. The optical properties in the interband transition region of c-MgxZn1xSe have been studied using SE [207,215]. The SE data analysis suggested that increasing x leads to a gradual increase in the E0/(E0 þ D0) and E1/(E1 þ D1) CP energies. (d) MgCdSe The optical properties of w-MgxCd1xSe (0 x 0.46) were investigated by optical absorption measurements at 300 K [216]. SE was also used to obtain the «(E) spectra for w-MgxCd1xSe in the range of 0.756.5 eV with x ¼ 0.15 and 0.29 [210] and in the range of 1.254.5 eV with x ¼ 00.40 [217]. (e) ZnCdSe The n(E) dispersion in c-ZnxCd1xSe has been measured by Peiris et al. [211,218]. These authors reported the first-order Sellmeier parameters as a function of x [211]. The n(E) dispersion calculated using these parameters are shown in Figure 10.40, together with the experimental ZnSe data [3]. The bold solid line also represents the first-order Sellmeier parameters for ZnSe obtained by Adachi [213]. A temperature shift of Dn/DT ¼ 1.0 104 K1 (T ¼ 50–300 K) has also been reported by analyzing laser emission wavelengths from a ZnxCd1xSe-based distributed feedback laser [219]. SE has been used to study the optical properties of c-ZnxCd1xSe by several groups [220– 223]. The samples used in these studies were epitaxial films grown by MBE on GaAs with x ¼ 0–1.0 [220], 0.75–1.0 [221] and 0.66–1.0 [222] and on InP with x ¼ 0.53 [223].

338

PROPERTIES OF SEMICONDUCTOR ALLOYS 3.0 2.9

n

2.8 2.7 2.6

c-CdSe

ZnSe

x=0

2.5 2.4 2.3 0.5

c-ZnxCd1-xSe

1.0

1.0

1.5

2.0 E (eV)

2.5

3.0

Figure 10.40 n(E) dispersion in the transparent region of c-ZnxCd1xSe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Peiris et al. [211]. The bold solid line (ZnSe) is also calculated from the first-order Sellmeier parameters reported by Adachi [213]. The c-CdSe (x ¼ 0) and ZnSe (x ¼ 1.0) data are taken from Adachi [3]

Suzuki and Adachi [224] used the MDF calculation to obtain a closed analytic formula for the optical constants of c-ZnxCd1xSe as a function of x. Figure 10.41 shows the MDFcalculated n(E) spectra in the region below and above the E0/(E0 þ D0) edge of c-ZnxCd1xSe with increments in x of 0.2 [224]. The solid and open circles represent the experimental data taken from Adachi [3] (ZnSe) and Holden et al. [223] (Zn0.53Cd0.47Se), respectively.

Figure 10.41 Theoretical n(E) spectra in the region below and above the E0/(E0 þ D0) edge of c-Znx Cd1xSe with increments in x of 0.2 at 300 K. The black and gray circles represent the experimental data for ZnSe and Zn0.53Cd0.47Se, respectively. [Reprinted with permission from K. Suzuki and S. Adachi, J. Appl. Phys. 83, 1018 (1998). Copyright (1998), American Institute of Physics]

(f) CdHgSe IR reflectivity spectra of c-CdxHg1xSe (x ¼ 0–0.32) have been reported by Kumazaki et al. [225]. They found that the measured reflectivity can be explained by the dynamic dielectric function constructed as the sum of the interband, intraband and phonon contributions.

OPTICAL PROPERTIES

339

The temperature and composition dependence of n in the transparent region of c-CdxHg1xSe has been determined by means of a fringe-spacing analysis [226]. The optical absorption properties near the fundamental absorption edge of c- and w-CdxHg1xSe have also been reported [226–229]. The fundamental reflectivity spectra for c-CdxHg1xSe have been measured [230]. The SE «(E) spectra for c-CdxHg1xSe (x ¼ 0–0.3) have also been measured in the 1.7–5.6 eV region at 300 K [231].

10.5.4 (II, II)–Te Ternary Alloy (a) BeZnTe The optical properties in the interband transition region of BexZn1xTe have been investigated using reflectivity [232]. The x dependence of E0 has been determined from this study. SE has also been used to measure «2(E) in BexZn1xTe [233–235]. (b) MgZnTe

n

The n(E) dispersion in c-MgxZn1xTe layers (0 x 0.67) grown on GaAs(100) by MBE has been determined from reflectivity measurements [236]. Figure 10.42 shows the n(E) dispersion calculated using first-order Sellmeier parameters [236], together with the experimental ZnTe data [3]. The bold solid line (ZnTe) has also been calculated using first-order Sellmeier parameters [213]. 3.3 3.2 3.1 3.0 2.9 2.8 2.7 2.6 2.5 2.4 2.3

0.5

c-MgxZn1-xTe x=0 (ZnTe)

0.7

0

0.5

1.0

1.5 2.0 E (eV)

2.5

3.0

Figure 10.42 n(E) dispersion in the transparent region of c-MgxZn1xTe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Liu et al. [236]. The bold solid line (ZnTe) is also calculated from the first-order Sellmeier parameters reported by Adachi [213]. The experimental data are taken from Adachi [3] (solid circles)

The optical absorption coefficients a(E) in the fundamental absorption edge of bulk c-MgxZn1xT crystals (0 x 0.48) grown by the Bridgman method have been measured at 4.2 K [237]. These results have been reproduced in Figure 10.43. The n ¼ 1 (1s) excitonic peak can be clearly seen at the E0 edge of each sample. SE measurements have been carried out on MBE-grown c-ZnxCd1xSe/GaAs(100) layers (0 x 0.52) [238]. The composition dependence of the excitonic E0, E0 þ D0 and E2 gaps has been determined in this study.

340

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.43 a(E) spectra in the fundamental absorption edge of c-MgxZn1xTe (0 x 0.48) at 4.2 K. [Reprinted with permission from S.-J. Chung et al., J. Phys. Chem. Solids 60, 799–805 (1999), Copyright (1999) Elsevier]

(c) MgCdTe The IR reflectivity spectra for c-MgxCd1xTe with x ¼ 00.6 have been measured in the range of 100–500 cm1 at 300 K [239]. The n(E) dispersion in c-MgxCd1xTe has also been measured at 4 K by Andre and Dang [240], at 77 and 300 K by Lugauer et al. [241] and at 300 K by Luttmann et al. [242]. Figure 10.44 shows the n(E) spectra calculated from first-order Sellmeier parameters by Luttmann et al. [242], together with the experimental CdTe n(E) data taken from Adachi [3]. 3.6 3.4

c-MgxCd1-xTe

n

3.2 3.0

x = 0 (CdTe)

0.5

2.8 1.0

2.6 2.4 2.2

0

0.5 1.0 1.5 2.0 2.5 3.0 3.5 E (eV)

Figure 10.44 n(E) dispersion in the transparent region of c-MgxZn1xTe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Luttmann et al. [242]. The experimental CdTe data are taken from Adachi [3]

SE measurements have been performed to determine the «(E) spectra for c-MgxCd1xTe [242–244]. The composition-dependent higher-order CPs, such as E1, E1 þ D1 and E2, have been determined from these «(E) spectra. (d) ZnCdTe The IR reflectivity in the reststrahlen region of ZnxCd1xTe has been measured by several authors [245–248]. The n(E) dispersion in ZnxCd1xTe has also been measured at room

OPTICAL PROPERTIES

341

3.3 3.2

0.8

ZnxCd1-xTe 0.5

3.1 n

0.3

3.0 2.9

x = 0 (CdTe)

1.0 (ZnTe)

2.8 2.7 0.5

1.0

1.5 E (eV)

2.0

2.5

Figure 10.45 n(E) dispersion in the transparent region of ZnxCd1xTe at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters [249]. The open circles represent the CdTe (x ¼ 0) and ZnTe (x ¼ 1.0) data taken from Adachi [3]

temperature in the 1.1–2.5 eV range by Adachi and Kimura [249]. The samples used by these authors were grown by the conventional Bridgman method. These results have been reproduced in Figure 10.45. The optical absorption spectra in the near-IR and mid-IR regions of ZnxCd1xTe have been measured at 300 K [250–252] and at 2 K [252]. The absorption coefficients a(E) are found to exhibit an exponential dependence on E according to the Urbach rule [251]. The room-temperature reflectivity spectra in the interband transition region of ZnxCd1xTe have been measured by several authors [253–256]. The R(E) spectra revealed the higherlying CPs, E0, E1, E1 þ D1, etc. The optical properties in the interband transition region of ZnxCd1xTe have also been investigated using SE [257–260]. The n(E) and k(E) spectra obtained by Adachi and Kimura have been reproduced in Figure 10.46 [257]. These spectra were parameterized to enable the calculation of the optical response in a ZnxCd1xTe alloy having an arbitrary composition x and photon energy E.

Figure 10.46 n(E) and k(E) spectra for ZnxCd1xTe with x ¼ 0, 0.3, 0.5, 0.8 and 1.0 at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Optical constants of Zn1xCdxTe ternary alloys: Experiment and modeling by S. Adachi and T. Kimura, 32, 3496. Copyright (1993), Institute of Pure and Applied Physics]

342

PROPERTIES OF SEMICONDUCTOR ALLOYS

(e) ZnHgTe The IR optical properties of ZnxHg1xTe have been studied by a number of authors [261–264]. The absorption coefficients a(E) in the fundamental absorption edge of ZnxHg1xTe have also been measured by several authors [264–266]. SE has been carried out on ZnxHg1xTe in the range between 0.75 and 5.7 eV by Castaing et al. [267]. (f) CdHgTe The optical properties in the reststrahlen region of CdxHg1xTe have been investigated by a number of groups [263,268–271]. The a(E) spectra in the IR region have also been measured by a number of authors [272–278]. An empirical formula for the intrinsic optical absorption coefficient in the Kane region is given by Chu et al. [279]. The n(E) dispersion in CdxHg1xTe has been measured at different temperatures from 77 up to 350 K [273,275,280,281]. Figure 10.47 shows the results obtained by Kucera [280]. Liu et al. [281] also obtained n(l, T) from transmittance interference spacing nðl; TÞ2 ¼ A þ

B 2

1ðC=lÞ

þ Dl2

ð10:13Þ

Figure 10.47 n(E) dispersion in CdxHg1xTe with x ¼ 0.180–1.000 at 300 K. [Reprinted with permission from Z. Kucera, Phys. Status Solidi A 100, 659–665 (1987), Copyright (1987) Wiley–VCH]

where l is the wavelength and A, B, C and D are fitting parameters which vary with composition x and temperature T. This formula can be used for x ¼ 0.200–0.443 at T ¼ 4.2–300 K. The formula can also be used with x 0.540 at different temperatures and with x ¼ 0.54–1.0 at room temperature. The fundamental reflectivity spectra in the interband transition region of CdxHg1xTe have been measured at 315 K by Gał azka ˛ and Kisiel [282] and at 115–300 K by Rodzik and Kisiel [283]. The optical properties of CdxHg1xTe have also been studied using SE in the 1.8–5.5 eV spectral region by Vi~ na et al. [284] and in the 1.5–6.0 eV region by Arwin and Aspnes [285]. The dependence of «(E) on T has been discussed by Kim and Sivananthan [286] and Johs et al. [287].

OPTICAL PROPERTIES

343

10.5.5 Zn–(VI, VI) Ternary Alloy (a) ZnOS A series of w-ZnOxS1x films with 0 x 1.0 were deposited by rf reactive sputtering on different substrates [288] and the composition dependence of E0 was then determined from optical transmission measurements (Figure 6.59(a)). (b) ZnSSe The IR reflectivity and absorption in c-ZnSxSe1x have been measured by several authors [289,290]. The n(E) and k(E) curves for c-ZnSxSe1x have also been determined from optical transmittance measurements [291]. Ozaki and Adachi [292] carried out MDF analysis to obtain a closed analytic formula for the optical constants of c-ZnSxSe1x as a function of x. Figure 10.48 shows the MDF-calculated n(E) dispersion in the E0/(E0 þ D0) region of c-ZnSxSe1x with increments in x of 0.1 [292].

Figure 10.48 n(E) dispersion in the transparent region of c-ZnSxSe1x with increments in x of 0.1 at 300 K. The n(E) curves are obtained from the MDF calculation. [Reprinted with permission from S. Ozaki and S. Adachi, J. Appl. Phys. 75, 7470 (1994). Copyright (1994), American Institute of Physics]

The low-temperature absorption coefficients a(E) in the E0 region of MOCVD-grown c-ZnSxSe1x layers were measured by Gebhard and Sch€otz [293]. The hydrostatic-pressure dependent a(E) spectra were also reported by the same authors [294]. The room-temperature R(E) spectra in the interband transition region of c-ZnSxSe1x were measured by Ebina et al. [295]. Several peaks related to the higher-lying CPs were determined as a function of x. The R values (0.3) are, however, considerably smaller than those obtained by Ozaki and Adachi [292], suggesting that the sample surfaces used by Ebina et al. were of poorer quality. Jans et al. [221] carried out SE measurements on MBE-grown c-ZnSxSe1x/GaAs samples. They reported only the «(E) spectrum for ZnS0.15Se0.85. Ozaki and Adachi [292] presented the MDF-calculated «(E) spectra in the 16 eV region of c-ZnSxSe1x with increments in x of 0.2. (c) ZnSTe A strongly nonlinear pressure dependence of the band gaps and large downward shifts of the CB edges as a function of x in c-ZnSxTe1x has been found from optical transmittance

344

PROPERTIES OF SEMICONDUCTOR ALLOYS

data [296] (Figure 6.59(c)). SE has also been used to determine the «(E) spectra in the 1.5–6.0 eV region of c-ZnSxTe1x films deposited by hot-wall epitaxy [297]. (d) ZnSeTe The optical properties in the reststrahlen region of ZnSexTe1x have been measured by several authors [298,299]. A series of ZnSexTe1x films with 0 x 1.0 were grown on GaAs(100) substrates by MBE to determine the x dependence of n(E) [300]. Ozaki and Adachi [301] used the MDF method to obtain a closed analytic formula for the optical constants of ZnSexTe1x as a function of x. Figure 10.49 shows the MDF-calculated n(E) dispersion in the E0/(E0 þ D0) region of ZnSexTe1x with increments in x of 0.1 [301].

Figure 10.49 n(E) dispersion in the transparent region of ZnSexTe1x with increments in x of 0.1 at 300 K. The n(E) curves are obtained from the MDF calculation. [Reprinted with permission from Jpn. J. Appl. Phys., Optical constants of ZnSexTe1x ternary alloys by S. Ozaki and S. Adachi, 32, 2620–2625. Copyright (1993), Japanese Society of Applied Physics]

The hydrostatic-pressure dependent a(E) spectra were measured by Wu et al. [302]. The first- and second-order pressure coefficients of the fundamental absorption edge were determined as a function of x. The fundamental reflectivity spectra in the interband transition region of ZnSexTe1x were measured at 300 K by Ebina et al. [303]. The CP energies, such as E0, E0 þ D0, E1, E1 þ D1 and E2, were determined as a function of x. It should be noted however, that the R values (0.4) obtained were considerably smaller than those reported by Ozaki and Adachi [301], suggesting that Ebina et al. had used sample surfaces of inferior quality [303]. Ozaki and Adachi [301] also reported the MDF-calculated «(E) spectra in the 1–6 eV region of ZnSexTe1x with increments in x of 0.1.

10.5.6 Cd–(VI, VI) Ternary Alloy (a) CdSSe The optical properties in the reststrahlen region of w-CdSxSe1x have been studied by several authors [304–307]. The n(E) dispersion in the transparent region of w-CdSxSe1x has been measured with 0 x 1.0 in the temperature range between 100 and 600 K by

OPTICAL PROPERTIES

345

Figure 10.50 n(E) dispersion in the transparent region of w-CdSxSe1x with x ¼ 0, 0.36, 0.58, 0.79, 0.92 and 1.00 at 300 K. The solid and open symbols correspond to those for E?c (no) and E||c (ne), respectively. [Reprinted with permission from M. P. Lisitsa, L. F. Gudymenko, V. N. Malinko, and S. F. Terekhova, Phys. Status Solidi 31, 389 (1969), Copyright (1969) Wiley–VCH]

Lisitsa et al. [308]. These authors presented the results in a variety of graphical and tabular forms. The n(E) data at 300 K have been reproduced in Figure 10.50. The natural birefringence ne(E||c) > no(E?c) is evident for all samples investigated. Femtosecond time-resolved refractive-index changes in CdS0.75Se0.25 and CdS have also been measured using a pump–probe deflection technique [309]. The n(E) curves for polycrystalline CdSxSe1x films deposited on quartz substrates by pulsed-laser ablation technique have also been reported [310]. The a(E) spectra in the E0 region of w-CdSxSe1x have been measured for polarizations E?c and E||c [311]. The a(E) spectra for polycrystalline CdSxSe1x samples have also been reported [310]. The UV reflectivity of w-CdSxSe1x single crystals has been investigated at 90 K using linearly polarized light [312]. The x-dependent CPs, such as E1, E00, E2 and E10, were determined and correlated with the electronic dipole transitions in the BZ. (b) CdSTe Long-wavelength IR spectroscopy has been used to study the lattice vibrations in CdSxTe1x [313]. The sphalerite–wurtzite phase transition is found to occur in the x ¼ 0.20–0.25 range. The optical constants, n and a, of flash-evaporated CdSxTe1x films with 0 x 1.0 have been determined from reflectance and transmittance measurements [314]. As expected, the n value at l ¼ 2 mm decreased with increasing x. Thin films of polycrystalline CdSxTe1x (0 x 1.0) have also been prepared by vacuum evaporation. The complex refractive indices n ¼ n þ ik for these films have been determined in the wavelength range of 250–3200 nm from reflectance and transmittance measurements [315]. SE has been used to determine the optical constants in the IR–UV spectral region of polycrystalline CdSxTe1x films (0 x x1.0) grown on borosilicate glasses by PLD [316]. A modified MDF is used to analyze the measured SE spectra.

346

PROPERTIES OF SEMICONDUCTOR ALLOYS

(c) CdSeTe The IR reflectivity for Bridgman-grown CdSxSe1x (0 x x1.0) was investigated by several authors [317,318]. The composition dependence of the phonon frequencies did not show any discontinuity when the crystal structure changed from zinc-blende to wurtzite. More recently, Feng et al. [319] undertook IR reflectivity studies on CdSxSe1x (x 0.36). The samples used were grown by the Bridgman method and were single crystals with the zinc-blende structure. Optical constants, such as n and a, for CdSxSe1x in the limited composition ranges have also been reported [320–322].

10.5.7 (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe The n(E) dispersion in MgxZn1xSySe1y/GaAs has been measured by several authors [323– 325]. These data showed that the smaller E0-gap material has a larger n value, as in many tetrahedral semiconductor alloys. The optical absorption in the fundamental absorption edge of MgxZn1xSySe1y/GaAs has also been measured by Lunz et al. [325]. SE has been used to determine the temperature dependence of E0 from 300 K to growth temperature in alloy compositions used in cladding layers and waveguides for blue–green light-emitting devices [326]. (b) MgZnSeTe The refractive index n at l ¼ 600 nm for MgxZn1xSeyTe1y/InP has been measured by Naniwae et al. [327]. The n value decreased almost linearly as the Mg content x increased in accordance with n ¼ 2.99–1.09x. The pressure-dependent absorption coefficients a(E) for MgxZn1xSeyTe1y have also been measured to investigate the band anticrossing effects [328], as popularly observed in dilute-nitride III–V alloys.

10.5.8 (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe The n(E) dispersion in BexMgyZn1xySe/GaP has been measured at 300 K using SE [329]. The n value at l ¼ 370 nm decreased almost linearly as the alloy E0 value increased in accordance with n ¼ 4.61–0.49E0. SE has also been used to determine the composition dependence of CPs in BexMgyZn1xySe/GaAs [330]. (b) BeZnCdSe SE has been used to characterize bulk BexZnyCd1xySe grown by the Bridgman method [331]. The first-order Sellmeier equation is used to model the experimental n(E) data in the transparent region of the bulk alloys. (c) MgZnCdSe The n(E) dispersion in the transparent region of MgxZnyCd1xySe/InP has been measured by Morita et al. [332] and Guo et al. [333]. The experimental n(E) data obtained by Guo et al. [333] have been reproduced in Figure 10.51. These data were obtained using a prism coupler

OPTICAL PROPERTIES

347

Figure 10.51 n(E) dispersion in the transparent region of MgxZnyCd1xySe/InP at 300 K. [Reprinted with permission from S. P. Guo, O. Maksimov, M. C. Tamargo, F. C. Peiris, and J. K. Furdyna, Appl. Phys. Lett. 77, 4107 (2000). Copyright (2000), American Institute of Physics]

technique. Peiris et al. [334] also reported the refractive-index step Dn between MgxZnyCd1xySe and ZnxCd1xSe at l ¼ 632.8 nm.

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] S. Adachi, Optical Properties of Crystalline and Amorphous Semiconductors: Materials and Fundamental Principles, Kluwer Academic, Boston, 1999. [3] S. Adachi, Optical Constants of Crystalline and Amorphous Semiconductors: Numerical Data and Graphical Information, Kluwer Academic, Boston, 1999. [4] W. Kissinger, M. Weidner, H. J. Osten, and M. Eichler, Appl. Phys. Lett. 65, 3356 (1994). [5] H. Lee, S. R. Kurtz, J. A. Floro, J. Strane, C. H. Seager, S. R. Lee, E. D. Jones, J. F. Nelson, T. Mayer, and S. T. Picraux, Jpn. J. Appl. Phys. 34, L1340 (1995). [6] J. S. Schrader, J. L. Huguenin-Love, R. J. Soukup, N. J. Ianno, C. L. Exstrom, S. A. Darveau, R. N. Udey, and V. L. Dalal, Sol. Ener. Mater. Sol. Cells 90, 2338 (2006). [7] K. Kolodzey, P. A. O’Neil, S. Zhang, B. A. Orner, K. Roe, K. M. Unruh, C. P. Swann, M. M. Waite, and S. I. Shah, Appl. Phys. Lett. 67, 1865 (1995). [8] M. Krishnamurthy, K. -K. Yang, and W. H. Weber, Appl. Phys. Lett. 69, 2572 (1996). [9] R. Braunstein, Phys. Rev. 130, 879 (1963). [10] R. Braunstein, Phys. Rev. 130, 869 (1963). [11] R. Braunstein, A. R. Moore, and F. Herman, Phys. Rev. 109, 695 (195). [12] C. Pickering and R. T. Carline, J. Appl. Phys. 75, 4642 (1994). [13] J. C. Tsang, V. P. Kesan, J. L. Freeouf, F. K. LeGoues, and S. S. Iyer, Phys. Rev. B 46, 6907 (1992). [14] G. He and H. A. Atwater, Phys. Rev. Lett. 79, 1937 (1997). [15] H. P. L. de Guevara, A. G. Rodrıguez, H. Navarro-Contreras, and M. A. Vidal, Appl. Phys. Lett. 84, 4532 (2004).

348

PROPERTIES OF SEMICONDUCTOR ALLOYS

[16] H. P. L. de Guevara, A. G. Rodrıguez, H. Navarro-Contreras, and M. A. Vidal, Appl. Phys. Lett. 91, 161909 (2007). [17] V. R. D’Costa, C. S. Cook, A. G. Birdwell, C. L. Littler, M. Canonico, S. Zollner, J. Kouvetakis, and J. Menendez, Phys. Rev. B 73, 125207 (2006). [18] L. V. Kulik, C. Guedj, M. W. Dashiell, J. Kolodzey, and A. Hairie, Phys. Rev. B 59, 15753 (1999). [19] B. A. Orner, J. Olowolafe, K. Roe, J. Kolodzey, T. Laursen, J. W. Mayer, and J. Spear, Appl. Phys. Lett. 69, 2557 (1996). [20] H. Lee, J. A. Floro, J. Strane, S. R. Lee, E. D. Jones, T. Mayer, and S. T. Picraux, Mater. Res. Soc. Symp. Proc. 379, 211 (1995). [21] B.-K. Yang, M. Krishnamurthy, and W. H. Weber, J. Appl. Phys. 84, 2011 (1998). [22] S. Zollner, J. Hildreth, R. Liu, P. Zaumseil, M. Weidner, and B. Tillack, J. Appl. Phys. 88, 4102 (2000). [23] P. Aella, C. Cook, J. Tolle, S. Zollner, A. V. G. Chizmeshya, and J. Kouvetakis, Appl. Phys. Lett. 84, 888 (2004). [24] T. Suzuki, H. Yaguchi, H. Okumura, Y. Ishida, and S. Yoshida, Jpn. J. Appl. Phys. 39, L497 (2000). [25] U. K€ohler, D. J. As, B. Sch€ottker, T. Frey, K. Lischka, J. Scheiner, S. Shokhovets, and R. Goldhahn, J. Appl. Phys. 85, 404 (1999). [26] K. Torii, N. Usukura, A. Nakamura, T. Sota, S. F. Chichibu, T. Kitamura, and H. Okumura, Appl. Phys. Lett. 82, 52 (2003). [27] R. Goldhahn, J. Scheiner, S. Shokhovets, T. Frey, U. K€ ohler, D. J. As, and K. Lischka, Appl. Phys. Lett. 76, 291 (2000). [28] Z. G. Hu, M. Strassburg, N. Dietz, A. G. U. Perera, A. Asghar, and I. T. Ferguson, Phys. Rev. B 72, 245326 (2005). [29] K. Kazan, P. Masri, and M. Sumiya, J. Appl. Phys. 100, 013508 (2006). [30] U. Tisch, B. Meyler, O. Katz, E. Finkman, and J. Salzman, J. Appl. Phys. 89, 2676 (2001). € ur, H. O. Everitt, F. Yun, and H. Morko , Phys. Status Solidi A 188, 793 € Ozg€ [31] G. Webb-Wood, U. (2001). [32] R. Hui, S. Taherion, Y. Wan, J. Li, S. X. Jin, J. Y. Lin, and H. X. Jiang, Appl. Phys. Lett. 82, 1326 (2003). [33] N. Antoine-Vincent, F. Natali, M. Mihailovic, A. Vasson, J. Leymarie, P. Disseix, D. Byrne, F. Semond, and J. Massies, J. Appl. Phys. 93, 5222 (2003). [34] N. A. Sanford, L. H. Robins, A. V. Davydov, A. Shapiro, D. V. Tsvetkov, A. V. Dmitriev, S. Keller, U. K. Mishra, and S. P. DenBaars, J. Appl. Phys. 94, 2980 (2003). [35] N. Antoine-Vincent, F. Natali, M. Mihailovic, P. Disseix, A. Vasson, J. Leymarie, D. Byrne, F. Semond, and J. Massies, Phys. Status Solidi A 195, 543 (2003). [36] F. Omnes, N. Marenco, B. Beaumont, P. de Mierry, E. Monroy, F. Calle, and E. Mu~ noz, J. Appl. Phys. 86, 5286 (1999). [37] H. Angerer, D. Brunner, F. Freudenberg, O. Ambacher, M. Stutzmann, R. H€ opler, T. Metzger, E. Born, G. Dollinger, A. Bergmaier, S. Karsch, and H. -J. K€ orner, Appl. Phys. Lett. 71, 1504 (1997). [38] M. Stutzmann, O. Ambacher, A. Cros, M. S. Brandt, H. Angerer, R. Dimitrov, N. Reinacher, T. Metzger, R. H€opler, D. Brunner, F. Freudenberg, R. Handschuh, and C. Deger, Mater. Sci. Eng. B 50, 212 (1997). [39] T. Wethkamp, K. Wilmers, N. Esser, W. Richter, O. Ambacher, H. Angerer, G. Jungk, R. L. Johnson, and M. Cardona, Thin Solid Films 313–314, 745 (1998). [40] C. Buchheim, R. Goldhahn, M. Rakel, C. Cobet, N. Esser, U. Rossow, D. Fuhrmann, and A. Hangleiter, Phys. Status Solidi B 242, 2610 (2005). [41] T. Kawashima, H. Yoshikawa, S. Adachi, S. Fuke, and K. Ohtsuka, J. Appl. Phys. 82, 3528 (1997). [42] A. Kasic, M. Schubert, J. Off, and F. Scholz, Appl. Phys. Lett. 78, 1526 (2001). [43] G. M. Laws, E. C. Larkins, I. Harrison, C. Molloy, and D. Somerford, J. Appl. Phys. 89, 1108 (2001).

OPTICAL PROPERTIES

349

[44] Q. Guo, T. Tanaka, M. Nishio, and H. Ogawa, Jpn. J. Appl. Phys. 42, L141 (2003). [45] W. Terashima, S. -B. Che, Y. Ishitani, and A. Yoshikawa, Jpn. J. Appl. Phys. 45, L539 (2006). [46] R. Goldhahn, P. Schley, A. T. Winzer, G. Gobsch, V. Cimalla, O. Ambacher, M. Rakel, C. Cobet, N. Esser, H. Lu, and W. J. Schaff, Phys. Status Solidi A 203, 42 (2006). [47] K. Osamura, S. Naka, and Y. Murakami, J. Appl. Phys. 46, 3432 (1975). [48] N. A. Sanford, A. Munkholm, M. R. Kramers, A. Shapiro, I. Levin, A. V. Davydov, S. Sayan, L. S. Wielunski, and T. E. Madey, Phys. Status Solidi C 2, 2783 (2005). [49] T. Nagatomo, T. Kuboyama, H. Minamino, and O. Omoto, Jpn. J. Appl. Phys. 28, L1334 (1989). [50] C. A. Parker, J. C. Roerts, S. M. Bedair, M. J. Reed, S. X. Liu, N. A. El-Masry, and L. H. Robins, Appl. Phys. Lett. 75, 2566 (1999). [51] W. Walukiewicz, J. W. Ager III, K. M. Yu, Z. Liliental-Weber, J. Wu, S. X. Li, R. E. Jones, and J. D. Denlinger, J. Phys. D: Appl. Phys. 39, R83 (2006). [52] J. Wagner, A. Ramakrishnan, D. Behr, H. Obloh, M. Kunzer, and K. -H. Bachem, Appl. Phys. Lett. 73, 1715 (1998). [53] M. H. Lee, K. J. Kim, and E. Oh, Solid State Commun. 114, 325 (2000). [54] V. J. Keast, A. J. Scott, M. J. Kappers, C. T. Foxon, and C. J. Humphreys, Phys. Rev. B 66, 125319 (2002). [55] G. Lucovsky, R. D. Burnham, and A. S. Alimonda, Phys. Rev. B 14, 2503 (1976). [56] A. Onton, M. R. Lorenz, J. M. Woodall, and R. J. Chicotka, J. Cryst. Growth 27, 166 (1974). [57] P. Dias, V. A. Mishurnyi, E. L. Portnoi, B. S. Ryvkin, and V. B. Smirnitskii, Sov. Tech. Phys. Lett. 3, 290 (1977). [58] J. M. Rodrıguez and G. Armelles, J. Appl. Phys. 69, 965 (1991). [59] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, D. H. Woo, and S. H. Kim, J. Appl. Phys. 87, 1287 (2000). [60] G. Lucovsky, M. H. Brodsky, M. F. Chen, R. J. Chicotka, and A. T. Ward, Phys. Rev. B 4, 1945 (1971). [61] E. Jahne, W. Pilz, M. Giehler, and L. Hildisch, Phys. Status Solidi B 91, 155 (1979). [62] A. Hassine, J. Sapriel, P. L. Berre, P. Legay, F. Alexandre, and G. Post, J. Appl. Phys. 77, 6569 (1995). [63] A. R. Go~ni, K. Syassen, K. Str€ossner, and M. Cardona, Phys. Rev. B 39, 3178 (1989). [64] H. Lee, D. Biswas, M. V. Klein, H. Morkoç, D. E. Aspnes, B. D. Choe, J. Kim, and C. O. Grifﬁths, J. Appl. Phys. 75, 5040 (1994). [65] M. Schubert, V. Gottschalch, C. M. Herzinger, H. Yao, P. G. Snyder, and J. A. Woollam, J. Appl. Phys. 77, 3416 (1995). [66] R. Ferrini, G. Zuizzetti, M. Patrini, A. Parisini, L. Tarricone, and B. Valenti, Eur. Phys. J. B 27, 449 (2002). [67] D. H. Levi, J. F. Geisz, and B. Johs, Proc. SPIE 5530, 326 (2004). [68] S. Adachi, J. Appl. Phys. 58, R1 (1985). [69] D. E. Aspnes, S. M. Kelso, R. A. Logan, and R. Bhat, J. Appl. Phys. 60, 754 (1986). [70] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties. World Scientific, Singapore, 1994. [71] R. P. Seisyan, V. A. Kosobukin, S. A. Vaganov, M. A. Markosov, T. S. Shamirzaev, K. S. Zhuravlev, A. K. Bakarov, and A. I. Toropov, Phys. Status Solidi C 2, 900 (2005). [72] R. G. Kaufman, G. R. Hulse, D. J. Vezzetti, A. L. Moretti, K. A. Stair, G. P. Devane, and T. E. Bird, J. Appl. Phys. 75, 8053 (1994). [73] J. -H. Shin, and Y. -H. Lee, J. Appl. Phys. 76, 8048 (1994). [74] R. J. Deri and M. A. Emanuel, J. Appl. Phys. 77, 4667 (1995). [75] Y. Kokubo and I. Ohta, J. Appl. Phys. 81, 2042 (1997). [76] S. Gehrsitz, F. K. Reinhart, C. Gourdon, N. Herres, A. Vonlanthen, and H. Sigg, J. Appl. Phys. 87, 7825 (2000).

350

PROPERTIES OF SEMICONDUCTOR ALLOYS

[77] Z. G. Hu, M. B. M. Rinzan, S. G. Matsik, A. G. U. Perera, G. Von Winckel, A. Stintz, and S. Krishna, J. Appl. Phys. 97, 093529 (2005). [78] C. H. Kuo, S. Anand, H. Fathollahnejad, R. Ramamurti, R. Droopad, and G. N. Maracas, J. Vac. Sci. Technol. B 13, 681 (1995). [79] S. -J. Cho, and P. G. Snyder, J. Vac. Sci. Technol. B 17, 2045 (1999). Matyas, Sov. Phys. Semicond. 13, 1194 (1979). [80] E. [81] P. Roura, M. Lopez-de Miguel A. Cornet, and J. R. Morante, J. Appl. Phys. 81, 6916 (1997). [82] M. J. Mondry, D. I. Babic, J. E. Bowers, and L. A. Coldren, IEEE Photon. Technol. Lett. 4, 627 (1992). [83] H. Asai and H. Iwamura, Inst. Phys. Conf. Ser. 145, 985 (1996). [84] J. -H. Baek, B. Lee, S. W. Choi, J. H. Lee, and E. -H. Lee, Appl. Phys. Lett. 68, 2355 (1996). [85] H. W. Dinges, H. Burkhard, R. L€osch, H. Nickel, and W. Schlapp, Appl. Surf. Sci. 54, 477 (1992). [86] L. I. Kamlet, F. L. Terry, Jr., Thin Solid Films 313–314, 177 (1998). [87] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992. [88] G. Yu, N. L. Rowell, D. J. Lockwood, and P. J. Poole, Appl. Phys. Lett. 81, 2175 (2002); erratum, ibid. 82, 1136 (2003). [89] G. Yu, N. L. Rowell, D. J. Lockwood, and P. J. Poole, Appl. Phys. Lett. 86, 221904 (2005). [90] D. J. Lockwood, G. Yu, N. L. Rowell, and P. J. Poole, J. Appl. Phys. 101, 113524 (2007). [91] G. W. Charache, D. M. DePoy, J. E. Raynolds, P. F. Baldasaro, K. E. Miyano, T. Holden, F. H. Pollak, P. R. Sharps, M. L. Timmons, C. B. Geller, W. Mannstadt, R. Asahi, A. J. Freeman, and W. Wolf, J. Appl. Phys. 86, 452 (1999). [92] T. Takagi, Jpn. J. Appl. Phys. 17, 1813 (1978). [93] T. J. Kim, T. H. Ghong, Y. D. Kim, D. E. Aspnes, T. Mori, T. Yao, and B. H. Koo, Phys. Rev. B 68, 115323 (2003). [94] T. J. Kim, T. H. Ghong, and Y. D. Kim, J. Kor. Phys. Soc. 44, 726 (2004). [95] R. T. Carline, C. Pickering, N. S. Garawal, D. Lancefield, L. K. Howard, and M. T. Emeny, Proc. SPIE 1678, 285 (1992). [96] V. A. Yakovlen, Mater. Res. Soc. Symp. Proc. 340, 373 (1994). [97] L. C. Andreani, D. D. Nova, S. D. Lernia, M. Geddo, G. Guizzetti, M. Patrini, C. Bocchi, A. Bosacchi, C. Ferrari, and S. Franchi, J. Appl. Phys. 78, 6745 (1995). [98] M. Geddo, G. Guizzetti, M. Patrini, T. Ciabattoni, L. Seravalli, P. Frigeri, and S. Franchi, Appl. Phys. Lett. 87, 263120 (2005). [99] G. Lucovsky, K. Y. Cheng, and G. L. Pearson, Phys. Rev. B 12, 4135 (1975). [100] N. Kitamura and T. Wada, Mater. Lett. 19, 105 (1994). [101] R. Ferrini, M. Galli, G. Guizzetti, M. Patrini, A. Bosacchi, S. Franchi, and R. Magnanini, Phys. Rev. B 56, 7549 (1997). [102] R. Ferrini, M. Patrini, and S. Franchi, J. Appl. Phys. 84, 4517 (1998). [103] C. Ance and A. N. Van Mau, J. Phys. C: Solid State Phys. 9, 1565 (1976). [104] A. Bignazzi, E. Grilli, M. Guzzi, C. Bocchi, A. Bosacchi, S. Franchi, and R. Magnanini, Phys. Rev. B 57, 2295 (1998). [105] S. Dilernia, M. Geddo, G. Guizzetti, M. Patrini, A. Bosacchi, S. Franchi, and R. Magnanini, Mat. Res. Soc. Symp. Proc. 406, 389 (1996). [106] S. G. Choi, C. J. Palmstrem, Y. D. Kim, S. L. Cooper, and D. E. Aspnes, J. Appl. Phys. 98, 104108 (2005). [107] M. H. Brodsky, G. Lucovsky, M. F. Chen, and T. S. Plaskett, Phys. Rev. B 2, 3303 (1970). [108] Z. C. Feng, S. Perkowitz, R. Rousina, and J. B. Webb, Can. J. Phys. 69, 386 (1991). [109] R. Rousina, C. Halpin, and J. B. Webb, J. Appl. Phys. 68, 2181 (1990). [110] S. Imai and S. Adachi, Jpn. J. Appl. Phys. 32, 3860 (1993). [111] G. Leibiger, V. Gottschalch, A. Kasic, and M. Schubert, Appl. Phys. Lett. 79, 3407 (2001).

OPTICAL PROPERTIES

351

[112] J. B. Wang, Z. F. Li, W. Lu, D. J. Chen, B. Shen, and Y. D. Zheng, J. Vac. Sci. Technol. A 22, 1956 (2004). [113] G. Y. Rudko, I. A. Buyanova, W. M. Chen, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 81, 3984 (2002). [114] I. A. Buyanova, M. Izadifard, A. Kasic, H. Arwin, W. M. Chen, H. P. Xin, Y. G. Hong, and C. W. Tu, Phys. Rev. B 70, 085209 (2004). [115] B. Fluegel, Y. Zhang, J. F. Geisz, and A. Mascarenhas, Phys. Rev. B 72, 073203 (2005). [116] G. Leibiger, V. Gottschalch, M. Schubert, G. Benndorf, and R. Schwabe, Phys. Rev. B 65, 245207 (2002). [117] K. Uesugi and I. Suemune, Jpn. J. Appl. Phys. 36, L1572 (1997). [118] R. Chtourou, F. Bousbih, S. B. Bouzid, F. F. Charfi, J. C. Harmand, G. Ungaro, and L. Largeau, Appl. Phys. Lett. 80, 2075 (2002). [119] U. Tisch, E. Finkman, and J. Salzman, Appl. Phys. Lett. 81, 463 (2002). [120] W. K. Hung, M. Y. Chern, Y. F. Chen, Z. L. Yang, and Y. S. Huang, Phys. Rev. B 62, 13028 (2000). M. Schubert, G. Leibiger, V. Gottschalch, and G. Wagner, J. Appl. Phys. 89, 294 (2001). [121] J. Sik, and M. Schubert, J. Appl. Phys. 89, 4927 [122] G. Leibiger, V. Gottschalch, B. Rheinl€ander, J. Sik, (2001). [123] P. H. Jefferson, T. D. Veal, L. F. J. Piper, B. R. Bennett, C. F. McConville, B. N. Murdin, L. Buckie, G. W. Smith, and T. Ashley, Appl. Phys. Lett. 89, 111921 (2006). [124] W. G. Bi and C. W. Yu, J. Appl. Phys. 80, 1934 (1996). [125] W. K. Hung, K. S. Cho, M. Y. Chern, Y. F. Chen, D. K. Shih, H. H. Lin, C. C. Lu, and T. R. Yang, Appl. Phys. Lett. 80, 796 (2002). [126] D. -K. Shih, H. -H. Lin, L. -W. Sung, T. -Y. Chu, and T. -R. Yang, Jpn. J. Appl. Phys. 42, 375 (2003). [127] H. Shimomura, T. Anan, and S. Sugou, J. Cryst. Growth 162, 121 (1996). [128] F. Saadallah, N. Yacoubi, F. Genty, and C. Alibert, J. Appl. Phys. 94, 5041 (2003). [129] G. D. Clark, Jr., N. Holonyak, Jr., Phys. Rev. B 156, 913 (1967). [130] H. C. Casey, Jr., J. Appl. Phys. 45, 2766 (1974). [131] A. N. Pikhtin, A. D. Yas’kov, Sov. Phys. Semicond. 14, 389 (1980). [132] R. J. Nelson, N. Holonyak, Jr., and W. O. Groves, Phys. Rev. B 13, 5415 (1976). [133] A. G. Thompson, J. C. Woolley, and M. Rubenstein, Can. J. Phys. 44, 2927 (1966). [134] K. J. Kim, M. H. Lee, J. H. Bahng, K. Shim, and B. D. Choe, J. Appl. Phys. 84, 3696 (1998). [135] G. Lucovsky and M. F. Chen, Solid State Commun. 8, 1397 (1970). [136] M. Yano, Y. Suzuki, T. Ishii, Y. Matsushita, and M. Kimata, Jpn. J. Appl. Phys. 17, 2091 (1978). [137] K. G. Merkel, V. M. Bright, M. A. Marciniak, C. L. A. Cerny, and M. O. Manasreh, Appl. Phys. Lett. 65, 2442 (1994). [138] R. Lukic-Zrnic, B. P. Gorman, R. J. Cottier, T. D. Golding, C. L. Littler, and A. G. Norman, J. Appl. Phys. 92, 6939 (2002). [139] N. N. Sirota and E. E. Matyas, Phys. Status Solidi A 4, K143 (1971). [140] R. Ferrini, M. Geddo, G. Guizzetti, M. Patrini, S. Franchi, C. Bocchi, F. Germini, A. Baraldi, and R. Magnanini, J. Appl. Phys. 86, 4706 (1999). [141] D. Serries, M. Peter, N. Herres, K. Winkler, and J. Wagner, J. Appl. Phys. 87, 8522 (2000). [142] N. P. Kekelidze, G. P. Kekelidze, and Z. D. Makharadze, J. Phys. Chem. Solids 34, 2117 (1973). [143] D. J. Lockwood, N. L. Rowell, and G. Yu, J. Appl. Phys. 102, 033512 (2007). [144] I. V. Bodnar, A. I. Lukomskii, and G. F. Smirnova, Phys. Status Solidi A 37, K173 (1976). [145] S. G. Choi, C. J. Palmstrøm, Y. D. Kim, D. E. Aspnes, H. J. Kim, and Y. -C. Chang, Appl. Phys. Lett. 91, 041917 (2007). [146] E. H. Reihlen, M. J. Jou, Z. M. Fang, and G. B. Stringfellow, J. Appl. Phys. 68, 4604 (1990). [147] N. L. Rowell, D. J. Lockwood, G. Yu, Y. Z. Gao, X. Y. Gong, M. Aoyama, and T. Yamaguchi, J. Vac. Sci. Technol. A 22, 935 (2004). [148] M. B. Thomas and J. C. Woolley, Can. J. Phys. 49, 2052 (1971). [149] W. Dobbelaere, J. D. Boeck, and G. Borghs, Appl. Phys. Lett. 55, 1856 (1989).

352

PROPERTIES OF SEMICONDUCTOR ALLOYS

[150] V. K. Dixit, B. Bansal, V. Venkataraman, H. L. Bhat, K. S. Chandrasekharan, and B. M. Arora, J. Appl. Phys. 96, 4989 (2004). [151] M. A. Marciniak, R. L. Hengehold, Y. K. Yeo, and G. W. Turner, J. Appl. Phys. 84, 480 (1998). [152] G. B. Stringfellow and P. E. Greene, J. Electrochem. Soc. 118, 805 (1971). [153] H. Y. Deng and N. Dai, Phys. Rev. B 73, 113102 (2006). [154] Y. Z. Gao, X. Y. Gong, and T. Yamaguchi, Jpn. J. Appl. Phys. 45, 5732 (2006). [155] T. Imanishi, A. Wakahara, S. M. Kim, H. Yonezu, and Y. Furukawa, Phys. Status Solidi A 202, 854 (2005). [156] G. Leibiger, V. Gottschalch, and M. Schubert, J. Appl. Phys. 90, 5951 (2001). [157] C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002). [158] T. Kitatani, M. Kondow, K. Shinoda, Y. Yazawa, and M. Okai, Jpn. J. Appl. Phys. 37, 753 (1998). [159] P. N. Sen and G. Lucovsky, Phys. Rev. B 12, 2998 (1975). [160] V. V. Kuznetsov, V. N. Razbegaev, S. El-Giziri, Sov. Phys. Semicond. 23, 552 (1989). [161] A. Mezerreg, C. Llinares, J. L. Lazzari, and A. Montaner, Thin Solid Films 221, 196 (1992). [162] C. Alibert, M. Skouri, A. Joullie, M. Benouna, and S. Sadiq, J. Appl. Phys. 69, 3208 (1991). [163] O. Blum, I. J. Fritz, L. R. Dawson, and T. J. Drummond, Electron. Lett. 31, 1247 (1995). [164] P. Swarup, R. K. Jain, S. N. Verma, S Charan,h. and D. M. Tandle, Phys. Status Solidi A 65, K183 (1981). [165] F. Fiedler and A. Schlachetzki, Solid-State Electron. 30, 73 (1987). [166] S. M. Kelso, D. E. Aspnes, M. A. Pollack, and R. E. Nahory, Phys. Rev. B 26, 6669 (1982). [167] S. G. Wallace, B. J. Robinson, P. Mascher, H. K. Haugen, D. A. Thompson, D. Dalacu, and L. Martinu, Appl. Phys. Lett. 76, 2791 (2000). [168] C. Pickering, J. Electron. Mater. 15, 51 (1986). [169] W. G. Bi, A. Z. Li, and S. S. Tan, Mat. Res. Soc. Symp. Proc. 216, 213 (1991). [170] S. Adachi, J. Appl. Phys. 61, 4869 (1987). [171] M. S. S. Loural, M. B. Z. Morosini, J. L. Herrera-Perez, A. A. G. Von Zuben, A. C. F. da Silveir, and N. B. Patel, Electron. Lett. 29, 1240 (1993). [172] T. Hofmann, G. Leibiger, V. Gottschalch, I. Pietzonka, and M. Schubert, Phys. Rev. B 64, 155206 (2001). [173] S. Adachi, H. Kato, A. Moki, and K. Ohtsuka, J. Appl. Phys. 75, 478 (1994). [174] H. Tanaka, Y. Kawamura, and H. Asahi, J. Appl. Phys. 59, 985 (1986). [175] S. Ozaki, S. Adachi, M. Sato, and K. Ohtsuka, J. Appl. Phys. 79, 439 (1996). [176] M. Schubert, J. A. Woollam, G. Leibiger, B. Rheinl€ander, I. Pietzonka, T. Sab, and V. Gottschalch, J. Appl. Phys. 86, 2025 (1999). [177] K. Masu, T. Mishima, S. Hiroi, M. Konagai, and K. Takahashi, J. Appl. Phys. 53, 7558 (1982). [178] P. Swarup, R. K. Jain, S. N. Verma, S. Charan, and D. M. Tandle, Phys. Status Solidi A 72, K189 (1982). [179] H. W. Dinges, H. Burkhard, R. L€osch, H. Nickel, and W. Schlapp, Mater. Sci. Eng. B 21, 174 (1993). [180] A. G. Belov, G. M. Zinger, M. A. II’in, Yu. N. Korchagin, E. P. Rashevskaya, and A. I. Ryskin, Sov. Phys. Solid State 22, 839 (1980). [181] N. P. Esina, N. V. Zotova, B. A. Matveev, L. D. Neulmina, N. M. Stus’, and G. N. Talalakin, Sov. Phys. Semicond. 15, 1372 (1981). [182] Y. R. Ryu, T. S. Lee, J. A. Lubguban, A. B. Corman, H. W. White, J. H. Leem, M. S. Han, Y. S. Park, C. J. Youn, and W. J. Kim, Appl. Phys. Lett. 88, 052103 (2006). [183] M. S. Han, J. H. Kim, T. S. Jeong, J. M. Park, C. J. Youn, J. H. Leem, and Y. R. Ryu, J. Cryst. Growth 303, 506 (2007). [184] J. Chen and W. Z. Shen, Appl. Phys. Lett. 83, 2154 (2003). [185] C. Bundesmann, A. Rahm, M. Lorenz, M. Grundmann, and M. Schubert, J. Appl. Phys. 99, 113504 (2006). [186] R. Schmidt, B. Rheinl€ander, M. Shubert, D. Spemann, T. Butz, J. Lenzner, E. M. Kaidashev, M. Lorenz, A. Rahm, H. C. Semmelhack, and M. Grundmann, Appl. Phys. Lett. 82, 2260 (2003).

OPTICAL PROPERTIES

353

€ ur, M. J. Bergmann, H. O. Everitt, A. K. Sharma, C. Jin, and € Ozg€ [187] C. W. Teng, J. F. Muth, U. J. Narayan, Appl. Phys. Lett. 76, 979 (2000). [188] R. Schmidt-Grund, A. Carstens, B. Rheinl€ander, D. Spemann, H. Hochmut, G. Zimmermann, M. Lorenz, M. Grundmann, C. M. Herzinger, and M. Schubert, J. Appl. Phys. 99, 123701 (2006). [189] P. Yu, H. Wu, N. Chen, T. Xu, Y. Lao, and J. Liang, Opt. Mater. 28, 271 (2006). [190] H. P. Zhou, W. Z. Shen, N. B. Chen, and H. Z. Wu, Appl. Phys. Lett. 85, 3723 (2004). [191] J. A. Sans and A. Segura, High Pressure Res. 24, 119 (2004). [192] J. H. Kang, Y. R. Park, and K. J. Kim, Solid State Commun. 115, 127 (2000). [193] R. Schmidt-Grund, M. Schubert, B. Rheinl€ander, D. Fritsch, H. Schmidt, E. M. Kaidashev, M. Lorenz, C. M. Herzinger, and M. Grundmann, Thin Solid Films 455–456, 500 (2004). [194] T. D. Kang, H. Lee, W. -I. Park, and G. -C. Yi, Thin Solid Films 455–456, 609 (2004). [195] H. Tampo, H. Shibata, K. Maejima, A. Yamada, K. Matsubara, P. Fons, S. Niki, T. Tainaka, C. Chiba, and H. Kanie, Appl. Phys. Lett. 91, 261907 (2007). [196] T. Makino, Y. Segawa, M. Kawasaki, A. Ohtomo, R. Shiroki, K. Tamura, T. Yasuda, and H. Koinuma, Appl. Phys. Lett. 78, 1237 (2001). [197] S. Y. Lee, Y. Li, J. -S. Lee, J. K. Lee, M. Nastasi, S. A. Crooker, Q. X. Jia, H. -S. Kang, and J. -S. Kang, Appl. Phys. Lett. 85, 218 (2004). [198] J. Ishihara, A. Nakamura, S. Shigemori, T. Aoki, and J. Temmyo, Appl. Surf. Sci. 244, 381 (2005). [199] X. J. Wang, I. A. Buyanova, W. M. Chen, M. Izadifard, S. Rawal, D. P. Norton S. J. Pearton, A. Osinsky, J. W. Dong, and A. Dabiran, Appl. Phys. Lett. 89, 151909 (2006). [200] H. C. Ong and J. Y. Dai, Appl. Phys. Lett. 81, 1444 (2002). [201] M. P. Lisitsa, M. Y. Valakh, and N. K. Konovets, Phys. Status Solidi 34, 269 (1969). [202] P. Chen, J. E. Nicholls, M. O’Neill, J. H. C. Hogg, B. Lunn, D. E. Ashenford, M. Fay, and A. G. Cullis, Semicond. Sci. Technol. 13, 1439 (1998). [203] M. R. Muhamad, Jpn. J. Appl. Phys. 32, 3385 (1993). [204] A. Beliveau and C. Carlone, Phys. Rev. B 41, 9860 (1990). [205] F. C. Peiris, U. Bindley, J. K. Furdyna, H. Kim, A. K. Ramdas, and M. Grimsditch, Appl. Phys. Lett. 79, 473 (2001). [206] K. Wilmers, T. Wethkamp, N. Esser, C. Cobet, W. Richter, V. Wagner, H. Lugauer, F. Fischer, T. Gerhard, M. Keim, and M. Cardona, J. Electron. Mater. 28, 670 (1999). [207] H. Lee, I. -Y. Kim, J. Powell, D. E. Aspnes, S. Lee, F. Peiris, and J. K. Furdyna, J. Appl. Phys. 88, 878 (2000). [208] A. Bukaluk, A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Łegowski, ˛ H. Me˛ czy nska, and J. Szatkowski, Appl. Surf. Sci. 175–176, 531 (2001). [209] A. A. Wronkowska, A. Wronkowski, F. Firszt, S. Łegowski, ˛ H. Me˛ czy nska, A. Marasek, and W. Paszkowicz, Phys. Status Solidi C 1, 641 (2004). [210] F. Firszt, A. A. Wronkowska, A. Wronkowski, S. Ł e˛ gowski, A. Marasek, H. M e˛ czy nska, M. Pawlak, W. Paszkowicz, K. Strzałkowski, and A. J. Zakrzewski, Cryst. Res. Technol. 40, 386 (2005). [211] F. C. Peiris, S. Lee, U. Bindley, and J. K. Furdyna, J. Appl. Phys. 86, 918 (1999). [212] B. Derkowska, B. Sahraoui, X. N. Phu, G. Glowacki, and W. Bala, Opt. Mater. 15, 199 (2000). [213] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [214] M. W€orz, E. Griebl, T. Reisinger, R. Flierl, B. Haserer, T. Semmler, T. Frey, and W. Gebhardt, Phys. Status Solidi B 202, 805 (1997). [215] K. J. Kim, M. H. Lee, J. H. Bahng, C. Y. Kwak, and E. Oh, Solid State Commun. 105, 17 (1998). [216] D. -H. Shin, C. -D. Kim, H. -H. Jang, S. -H. Choe, D. -T. Kim, C. -S. Yoon, and W. -T. Kim, J. Cryst. Growth 177, 167 (1997). [217] A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Łegowski, ˛ H. M e˛ czy nska, and J. Szatkowski, Vacuum 63, 233 (2001). [218] F. C. Peiris, S. Lee, U. Bindley, and J. K. Furdyna, J. Appl. Phys. 84, 5194 (1998).

354

PROPERTIES OF SEMICONDUCTOR ALLOYS

[219] M. Illing, G. Bacher, A. Forchel, D. Hommel, B. Jobst, and G. Landwehr, Appl. Phys. Lett. 67, 1 (1995). [220] Y. D. Kim, M. V. Klein, S. F. Ren, Y. C. Chang, H. Luo, N. Samarthj, and J. K. Furdyna, Phys. Rev. B 49, 7262 (1994). [221] J. C. Jans, J. Petruzzello, J. M. Gaines, and D. J. Olego, Proc. SPIE 1985, 260 (1993). [222] J. Lee, F. Flack, N. Samarth, and R. W. Collins, Appl. Opt. 36, 5372 (1997). [223] T. Holden, P. Ram, F. H. Pollak, and J. L. Freeouf, Phys. Rev. B 56, 4037 (1997). [224] K. Suzuki and S. Adachi, J. Appl. Phys. 83, 1018 (1998). [225] K. Kumazaki, N. Nishiguchi, and M. Cardona, Solid State Commun. 58, 425 (1986). [226] C. J. Summers and J. G. Broerman, Phys. Rev. B 21, 559 (1980). [227] P. S. Kireev and V. V. Volkov, Sov. Phys. Semicond. 7, 949 (1974). [228] N. Himei and J. Muto, J. Mater. Sci.: Mater. Electron. 11, 145 (2000). [229] V. B. Pujari, S. H. Mane, V. S. Karande, J. S. Dargad, and L. P. Deshmukh, Mater. Chem. Phys. 83, 10 (2004). [230] I. N. Borisov, P. S. Kireev, V. V. Mikhailin, and V. M. Bezborodova, Sov. Phys. Semicond. 5, 734 (1971). [231] K. Kumazaki, L. Vi~na, C. Umbach, and M. Cardona, Phys. Status Solidi B 156, 371 (1989). [232] O. Maksimov and M. C. Tamargo, Appl. Phys. Lett. 79, 782 (2001). [233] M. R. Buckley, F. C. Peiris, O. Maksimov, M. Mu~ noz, and M. C. Tamargo, Appl. Phys. Lett. 81, 5156 (2002). [234] M. Mu~noz, O. Maksimov, M. C. Tamargo, M. R. Buckley, and F. C. Peiris, Phys. Status Solidi C 1, 706 (2004). [235] J. S. de Almeida, and R. Ahuja, Appl. Phys. Lett. 89, 061913 (2006). [236] X. Liu, U. Bindley, Y. Sasaki, and J. K. Furdyna, J. Appl. Phys. 91, 2859 (2002). [237] S. -J. Chung, Y. Kwon, C. -S. Yoon, B. -H. Kim, D. Cha, C. -D. Kim, W. -T. Kim, and C. U. Hong, J. Phys. Chem. Solids 60, 799 (1999). [238] A. J. Franz, F. C. Peiris, X. Liu, U. Bindley, and J. K. Furdyna, Phys. Status Solidi B 241, 507 (2004). [239] S. Nakamura, T. Fukumoto, A. Mitsuishi, and K. Itoh, J. Phys. Soc. Jpn 35, 1437 (1973). [240] R. Andre and L. S. Dang, J. Appl. Phys. 82, 5086 (1997). [241] H. -J. Lugauer, F. Fischer, T. Litz, A. Waag, D. Hommel, and G. Landwehr, Semicond. Sci. Technol. 9, 1567 (1994). [242] M. Luttmann, F. Bertin, and A. Chabli, J. Appl. Phys. 78, 3387 (1995). [243] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, I. Miotkowski, and A. K. Ramdas, Appl. Phys. Lett. 71, 249 (1997). [244] Y. S. Ihn, T. J. Kim, T. H. Ghong, Y. D. Kim, D. E. Aspnes, and J. Kossut, Thin Solid Films 455–456, 222 (2004). [245] H. Harada and S. Narita, J. Phys. Soc. Jpn 30, 1628 (1971). [246] L. K. Vodop’yanov, E. A. Vinogradov, A. M. Blinov, and V. A. Rukavishnikov, Sov. Phys. Solid State 14, 219 (1972). [247] S. Perkowitz, L. S. Kim, and Z. C. Feng, Phys. Rev. B 42, 1455 (1990). [248] D. N. Talwar, Z. C. Feng, and P. Becla, Phys. Rev. B 48, 17064 (1993). [249] S. Adachi and T. Kimura, Jpn. J. Appl. Phys. 32, 3866 (1993). [250] A. Ebina, K. Saito, and T. Takahashi, J. Appl. Phys. 44, 3659 (1973). [251] A. J. Syllaios, P. -K. Liao, B. J. Greene, H. F. Schaake, H. -Y. Liu, and G. Westphal, J. Electron. Mater. 26, 567 (1997). [252] D. Ohlmann, M. Mazilu, R. Levy, and B. H€onerlage, J. Appl. Phys. 82, 1355 (1997). [253] A. Kisiel, Acta Phys. Polon. A 38, 691 (1970). [254] K. Saito, A. Ebina, and T. Takahashi, Solid State Commun. 11, 841 (1972). [255] S. G. Kroitoru, O. G. Maksimova, and V. V. Sobolev, Sov. Phys. Semicond. 9, 1191 (1976). [256] V. V. Sovolev, O. G. Maksimova, and S. G. Kroitoru, Phys. Status Solidi B 103, 499 (1981).

OPTICAL PROPERTIES [257] [258] [259] [260] [261] [262] [263] [264] [265] [266] [267] [268] [269] [270] [271] [272] [273] [274] [275] [276] [277] [278] [279] [280] [281] [282] [283] [284] [285] [286] [287] [288] [289] [290] [291] [292] [293] [294] [295] [296] [297] [298]

355

S. Adachi and T. Kimura, Jpn. J. Appl. Phys. 32, 3496 (1993). O. Castaing, R. Granger, J. T. Benhlal, and R. Triboulet, J. Phys.: Condens. Matter 8, 5757 (1996). E. M. Larramendi, E. Puron, and O. de Melo, Semicond. Sci. Technol. 17, 8 (2002). P. D. Paulson, B. E. McCandless, and R. W. Birkmire, J. Appl. Phys. 95, 3010 (2004). G. L. Bastard, R. Granger, S. Rolland, Y. Marqueton, and R. Triboulet, J. Phys. (France) 50, 3223 (1989). M. P. Volz, F. R. Szofran, S. L. Lehoczky, and C. -H. Su, Solid State Commun. 75, 943 (1990). D. Bagot, R. Granger, and S. Rolland, Phys. Status Solidi B 183, 395 (1994). C. -H. Wu, D. -Y. Chu, C. -Y. Sun, and T. -R. Yang, Jpn. J. Appl. Phys. 34, 4687 (1995). B. Toulouse, R. Granger, S. Rolland, and R. Triboulet, J. Phys. (France) 48, 247 (1987). F. El-Akkad, and A. R. Farhan, J. Phys. D: Appl. Phys. 28, 1958 (1995). O. Castaing, J. T. Benhlal, R. Granger, and R. Triboulet, J. Phys. I (France) 6, 907 (1996). J. Baars and F. Sorger, Solid State Commun. 10, 875 (1972). D. N. Talwar and M. Vandevyver, J. Appl. Phys. 56, 1601 (1984). S. P. Kozyrev, V. N. Pyrkov, L. K. Vodop’yanov, Sov. Phys. Solid State 34, 1984 (1992). S. P. Kozyrev, L. K. Vodopyanov, and R. Triboulet, Phys. Rev. B 58, 1374 (1998). M. W. Scott, J. Appl. Phys. 40, 4077 (1969). E. Finkman and Y. Nemirovsky, J. Appl. Phys. 50, 4356 (1979). L. D. Saginov, V. P. Ponomarenko, V. A. Fedirko, and V. I. Stafeev, Sov. Phys. Semicond. 16, 298 (1982). E. Finkman and S. E. Schacham, J. Appl. Phys. 56, 2896 (1984). J. Chu, Z. Mi, and D. Tang, J. Appl. Phys. 71, 3955 (1992). B. Li, J. H. Chu, Y. Chang, Y. S. Gui, and D. Y. Tang, Infrared Phys. Technol. 37, 525 (1996). V. Nathan, J. Appl. Phys. 83, 2812 (1998). J. Chu, B. Li, and D. Tang, J. Appl. Phys. 75, 1234 (1994). Z. Kucera, Phys. Status Solidi A 100, 659 (1987). K. Liu, J. H. Chu, and D. Y. Tang, J. Appl. Phys. 75, 4176 (1994). R. R. Gał azka ˛ and A. Kisiel, Phys. Status Solidi 34, 63 (1969). A. Rodzik and A. Kisiel, J. Phys. C: Solid State Phys. 16, 203 (1983). L. Vi~na, C. Umbach, M. Cardona, and L. Vodopyanov, Phys. Rev. B 29, 6752 (1984). H. Arwin and D. E. Aspnes, J. Vac. Sci. Technol. A 2, 1316 (1984). C. C. Kim and S. Sivananthan, J. Electron. Mater. 26, 561 (1997). B. Johs, C. M. Herzinger, J. H. Dinan, A. Cornfeld, and J. D. Benson, Thin Solid Films 313–314, 137 (1998). B. K. Meyer, A. Polity, B. Farangis, Y. He, D. Hasselkamp, T. Kr€amer, and C. Wang, Appl. Phys. Lett. 85, 4929 (2004). O. Brafman, I. F. Chang, G. Lengyel, S. S. Mitra, E. Carnall, Jr., Phys. Rev. Lett. 19, 1120 (1967). D. Schmeltzer, R. Beserman, and D. Slamovits, Phys. Rev. B 22, 4038 (1980). M. Ambrico, D. Smaldone, C. Spezzacatena, V. Stagno, G. Perna, and V. Capozzi, Semicond. Sci. Technol. 13, 1446 (1998). S. Ozaki and S. Adachi, J. Appl. Phys. 75, 7470 (1994). W. Gebhard, G. Sch€otz, in Properties of Wide Bandgap IIVI Semiconductors, EMIS Datareviews Series No. 17 (edited by R. Bhargava), INSPEC (IEE), London, 1997, p. 113. E. Griebl, G. F. Sch€otz, C. Birzer, W. Kerner, T. Reisinger, B. Hahn, and W. Gebhardt, Acta Phys. Polon. A 88, 995 (1995). A. Ebina, E. Fukunaga, and T. Takahashi, Phys. Rev. B 10, 2495 (1974). W. Walukiewicz, W. Shan, K. M. Yu, J. W. Ager III, E. E. Haller, I. Miotkowski, M. J. Seong, H. Alawadhi, and A. K. Ramdas, Phys. Rev. Lett. 85, 1552 (2000). C. Y. Bang, M. S. Lee, T. J. Kim, Y. D. Kim, D. E. Aspnes, Y. M. Yu, B. O, and Y. D. Choi, J. Kor. Phys. Soc. 39, 462 (2001). V. M. Burlakov, A. P. Litvinchuk, and V. N. Pyrkov, Sov. Phys. Solid State 27, 131 (1985).

356 [299] [300] [301] [302] [303] [304] [305] [306] [307] [308] [309] [310] [311] [312] [313] [314] [315] [316] [317] [318] [319] [320] [321] [322] [323] [324] [325] [326] [327] [328] [329] [330] [331] [332] [333] [334]

PROPERTIES OF SEMICONDUCTOR ALLOYS T. R. Yang and C. C. Lu, Physica B 284–288, 1187 (2000). F. C. Peiris, U. Bindley, and J. K. Furdyna, J. Electron. Mater. 30, 677 (2001). S. Ozaki and S. Adachi, Jpn. J. Appl. Phys. 32, 2620 (1993). J. Wu, W. Walukiewicz, K. M. Yu, W. Shan, J. W. Ager III, E. E. Haller, I. Miotkowski, A. K. Ramdas, and C. -H. Su, Phys. Rev. B 68, 033206 (2003). A. Ebina, M. Yamamoto, and T. Takahashi, Phys. Rev. B 6, 3786 (1972). J. F. Parrish, C. H. Perry, O. Brafman, I. F. Chang and S. S. Mitra, in II–VI Semiconducting Compounds (edited by D. G. Thomas), Benjamin, New York, 1967, p. 1164. H. W. Verleur and A. S. Barker, Jr., Phys. Rev. 155, 750 (1967). R. Beserman and M. Balkanski, Phys. Rev. B 1, 608 (1970). R. Beserman, Solid State Commun. 23, 323 (1977). M. P. Lisitsa, L. F. Gudymenko, V. N. Malinko, and S. F. Terekhova, Phys. Status Solidi 31, 389 (1969). E. C. Fox, E. J. Canto-Said, and H. M. van Driel, Appl. Phys. Lett. 59, 1878 (1991). G. Perna, S. Pagliara, V. Capozzi, M. Ambrico, and T. Ligonzo, Thin Solid Films 349, 220 (1999). M. S. Brodin, M. V. Kurik, and S. P. Yurtsenyuk, Sov. Phys. Solid State 7, 2516 (1966). R. L. Hengehold and C. R. Fraime, Phys. Rev. 174, 808 (1968). Y. A. Mityagin, V. G. Plotnichenko, L. K. Vodop’yanov, and L. D. Budennaya, Sov. Phys. Solid State 19, 1811 (1977). K. Ohata, J. Saraie, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1641 (1973). D. A. Wood, D. W. Lane, K. D. Rogers, and J. A. Coath, J. Electron. Mater. 28, 1403 (1999). K. Wei, F. H. Pollak, J. L. Freeouf, D. Shvydka, and A. D. Compaan, J. Appl. Phys. 85, 7418 (1999). E. A. Vinogradov, L. K. Vodop’yanov, and G. S. Oleinik, Sov. Phys. Solid State 15, 322 (1973). M. Gorska and W. Nazarewicz, Phys. Status Solidi B 65, 193 (1974). Z. C. Feng, P. Becla, L. S. Kim, S. Perkowitz, Y. P. Feng, H. C. Poon, K. P. Williams, and G. D. Pitt, J. Cryst. Growth 138, 239 (1994). M. Neumann-Spallart, E. Galun, G. Hodes, C. Levy-Clement, Y. Marfaing, E. Muranevich, and R. Tenne, J. Appl. Phys. 73, 7753 (1993). S. Cohen, R. Weil, and E. Muranevich, J. Appl. Phys. 76, 593 (1994). M. M. El-Nahass, A. A. M. Farag, and H. E. A. El-Sayed, Appl. Phys. A 77, 819 (2003). H. Okuyama, K. Nakano, T. Miyazima, and K. Akimoto, Jpn. J. Appl. Phys. 30, L1620 (1991). M. Ukita, H. Okuyama, M. Ozawa, A. Ishibashi, K. Akimoto, and Y. Mori, Appl. Phys. Lett. 63, 2082 (1993). U. Lunz, B. Jobst, S. Einfeldt, C. R. Becker, D. Hommel, and G. Landwehr, J. Appl. Phys. 77, 5377 (1995). U. Lunz, C. Schumacher, J. N€urnberger, K. Sch€ ull, A. Gerhard, U. Sch€ ussler, B. Jobst, W. Faschinger, and G. Landwehr, Semicond. Sci. Technol. 12, 970 (1997). K. Naniwae, H. Iwata, and K. Yashiki, Appl. Phys. Lett. 74, 3984 (1999). J. Wu, W. Walukiewicz, K. M. Yu, J. W. Ager III, W. Shan, E. E. Haller, I. Miotkowski, A. K. Ramdas, and S. Miotkowska, Appl. Phys. Lett. 80, 34 (2002). Y. Niiyama and M. Watanabe, Semicond. Sci. Technol. 20, 1187 (2005). V. Wagner, A. Fleszar, J. Geurts, G. Reusher, M. Keim, A. Waag, G. Landwehr, K. Wilmers, N. Esser, and W. Richter, J. Cryst. Growth 214/215, 340 (2000). A. A. Wronkowska, F. Firszt, H. Arwin, A. Wronkowski, M. Wakula, K. Strzalkowski, and W. Paszkowicz, Phys. Status Solidi C 3, 1193 (2006). T. Morita, H. Shinbo, H. Shinbo, T. Nagano, I. Nomura, A. Kikuchi, and K. Kishino, J. Appl. Phys. 81, 7575 (1997). S. P. Guo, O. Maksimov, M. C. Tamargo, F. C. Peiris, and J. K. Furdyna, Appl. Phys. Lett. 77, 4107 (2000). F. C. Peiris, J. K. Furdyna, S. P. Guo, and M. C. Tamargo, J. Appl. Phys. 89, 3748 (2001).

11 Elasto-optic, Electro-optic and Nonlinear Optical Properties 11.1 ELASTO-OPTIC EFFECT 11.1.1 Group-IV Semiconductor Alloy Data relating to elasto-optic behavior plays an important role not only in the design of elasto-optic devices, such as light modulators, deflectors and switches, but also in the analysis of lattice-mismatched semiconductor heterostructures. Photoelasticity is dependent on wavelength [1–4]. The photoelastic coefficient in 6H-SiC has been measured by Geidur [5]. Since the fundamental absorption edge of 6H-SiC is an indirect band gap, its contribution to the photoelasticity is negligibly small. Neither theoretical nor experimental studies relating to photoelasticity have been carried out on any group-IV semiconductor alloy.

11.1.2 III–V Semiconductor Alloy A method for calculating the photoelastic coefficients in III–V semiconductors has been described by Adachi and Oe [6]. This model was applied to AlxGa1xAs and GaxIn1xPyAs1y/ InP. The photoelastic coefficient ape for AlxGa1xAs under X||[100] stress has been reproduced in Figure 11.1. The black and gray circles correspond to the experimental data for GaAs (x ¼ 0) and Al0.5Ga0.5As, respectively. The definition of ape can be found in Adachi [1]. More recently, Kikkarin et al. [7] have calculated the spectral dependence of the photoelastic constants, p11, p12 and p44, for AlxGa1xAs with x up to 0.3. They also discussed the acousto-optic interaction in AlxGa1xAs/GaAs waveguides.

11.1.3 II–VI Semiconductor Alloy The photoelastic constants pij can be determined from the Brillouin scattering crosssections [1]. Ziobrowski et al. [8] used Brillouin scattering on BexZn1xSe and obtained pij at l ¼ 488 nm (0 x 0.25). Adachi and Hamaguchi [9] carried out resonant Brillouin scattering measurements on ZnxCd1xTe and obtained the spectral dependence of p44 for x ¼ 0.65 and 0.80. The data suggest that the sign for p44 in ZnxCd1xTe is negative in the region remote from the E0 edge and becomes positive when the wavelength approaches the band edge, as in ZnTe and CdTe [4].

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

358

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 11.1 Photoelastic coefficient ape for AlxGa1xAs with increments in x of 0.2. The black and gray circles correspond to the experimental data for GaAs (x ¼ 0) and Al0.5Ga0.5As, respectively. [Reprinted with permission from S. Adachi and K. Oe, J. Appl. Phys. 54, 6620 (1983). Copyright (1983), American Institute of Physics]

11.2 LINEAR ELECTRO-OPTIC CONSTANT 11.2.1 Group-IV Semiconductor Alloy Principally, the diamond lattice shows no linear electro-optic effect [1]. The linear electro-optic constant r41 for 3C-SiC has been reported to be 2.7 0.5 pm/Vat l ¼ 632.8 nm [10]. There is an ordered alloy phase in SixGe1x (Section 1.3.2) and this phase will exhibit a linear electrooptic effect [11], but no data are available at present.

11.2.2 III–V Semiconductor Alloy The linear electro-optic effect in AlxGa1xAs has been studied by Glick et al. [12]. They measured the electro-optic phase difference in an Al0.17Ga0.83As waveguide and determined r41 at l ¼ 1.1523 mm, as shown in Table 11.1. Bach et al. [13] have measured r41 for GaxIn1xPyAs1y/InP (y ¼ 0.20 and 0.34). The values they obtained are summarized in Table 11.1. Figure 11.2 also shows the theoretical r41 dispersion obtained by Adachi and Oe [14], together with the data produced by Bach et al. (y ¼ 0.34) [13]. It can be seen that the theoretical r41 curve shows strong dispersion near E0 (l 1.1 mm). This curve was obtained from an electric-field-induced modulation of the electronic energy-band structure.

11.2.3 II–VI Semiconductor Alloy The linear electro-optic constant r41 at l ¼ 1.5 mm of Bridgman-grown Zn0.1Cd0.9Te has been measured by Zappettini et al. [15] (see Table 11.1). The implementation of a Zn0.1Cd0.9Tebased electro-optic switch which reaches 30 dB of extinction ratio and sub millisecond response time has also been presented by the same authors.

ELASTO-OPTIC, ELECTRO-OPTIC AND NONLINEAR OPTICAL PROPERTIES

359

Table 11.1 Linear electro-optic constant r41 for some III–V and II–VI semiconductor alloys. S ¼ clamped value System

Alloy

x (y)

III–V

AlxGa1xAs

0 0.17 0.20 (y) 0.34 (y) 0.34 (y) 1.00 (y)

GaxIn1xPyAs1y/InP

II–VI

ZnxCd1xTe

0 0.1 1.0

r41 (pm/V)

l (mm)

Comments

1.80a 1.43b 1.34c 1.43c 1.44c 1.68a

10.6 1.1523 1.32 1.25 1.32 1.50

S

10.6 1.5 10.6

S (|r41|) S (|r41|) S (|r41|)

4.1a 4.3d 3.9a

S

S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors. John Wiley & Sons, Ltd, Chichester, 2005 M. Glick et al., J. Appl. Phys. 63, 5877 (1988) c H. G. Bach et al., Appl. Phys. Lett. 42, 692 (1983) d A. Zappettini et al., J. Electron. Mater. 30, 743 (2001) a b

Figure 11.2 Theoretical r41 and R11R12 curves along with the experimental data of Bach et al. [13] for GaxIn1xPyAs1y/InP with y ¼ 0.34. [Reprinted with permission from S. Adachi and K. Oe, J. Appl. Phys. 56, 1499 (1984). Copyright (1984), American Institute of Physics]

The electro-optic constants rij of w-CdSxSe1x have been measured by several authors [16,17]. The results obtained by Baldassarre et al. [16] are r13 ¼ 1.5 pm/Vand r33 ¼ 2.4 pm/V at l ¼ 632.8 nm for x ¼ 0.75. More recently, Bini and Razzetti [17] reported the unclamped electro-optic constant T rcT ¼ r13

3 no T r33 ne

ð11:1Þ

to be 5.81 0.03 pm/V for x ¼ 0.5, where no and ne are, respectively, the ordinary and extraordinary refractive indices and rijT is the unclamped electro-optic tensor component [14]. These authors also obtained rcT ¼ 6:45 0:03 pm=V for w-CdS and 7.23 0.04 pm/V for

360

PROPERTIES OF SEMICONDUCTOR ALLOYS

w-CdSe. A smaller alloy value than those of the endpoint binaries is considered to be due to the microscopic strains present in the alloy.

11.3 QUADRATIC ELECTRO-OPTIC CONSTANT 11.3.1 Group-IV Semiconductor Alloy No detailed data are available for group-IV semiconductor alloys.

11.3.2 III–V Semiconductor Alloy Bach et al. [13] have studied the quadratic electro-optic effect in GaxIn1xPyAs1y/InP double-heterostructure waveguides. They obtained the quadratic electro-optic constants R11 R12 ¼ 0.8 1020 m2/V2 at l ¼ 1.32 mm for y ¼ 0.20 and R11 R12 ¼ 5.8 1020 (3.1 1020) m2/V2 at l ¼ 1.25 (1.32) mm for y ¼ 0.35. These results (y ¼ 0.35) are shown in Figure 11.2, together with the theoretical R11 R12 values calculated by Adachi and Oe [18]. It can be seen that the quadratic electro-optic constant R11 R12 shows very strong dispersion compared with the linear electro-optic constant (r41).

11.3.3 II–VI Semiconductor Alloy No detailed data are available for II–VI semiconductor alloys.

11.4 FRANZ–KELDYSH EFFECT 11.4.1 Group-IV Semiconductor Alloy Although the Franz–Keldysh effect in the indirect absorption edge of SiC has been discussed [19], no detailed data are available for group-IV semiconductor alloys.

11.4.2 III–V Semiconductor Alloy To our knowledge, there have been no publications relating to the direct measurement of the absorption edge shift in AlxGa1xAs under an applied electric field. The Franz–Keldysh effect in GaxIn1xPyAs1y/InP has been studied experimentally by several authors [13,20–22]. The change in the optical absorption coefficient Da observed in InP/GaInPAs/InP p-i-n double heterostructures [22] is found to be comparable with that obtained from the quantum-confined Stark effect (103 cm1).

11.4.3 II–VI Semiconductor Alloy Samuel et al. [23] measured the absorption coefficients near the fundamental absorption edge of ZnxCd1xSe and CdSxSe1x. They found that most of the results can be explained by the Dow–Redfield theory of the internal Franz–Keldysh effect. An enhancement of the two-photon

ELASTO-OPTIC, ELECTRO-OPTIC AND NONLINEAR OPTICAL PROPERTIES

361

absorption coefficient has also been observed to occur in the space charge region of the CdxHg1xTe p-n junction, which can be attributed to the Franz–Keldysh effect induced by the built-in electric field [24].

11.5 NONLINEAR OPTICAL CONSTANT 11.5.1 Group-IV semiconductor alloy The independent non-vanishing tensor elements of the nonlinear optical constants for semiconductors of certain symmetry classes are given in [1]. Principally, the diamond lattice does not show a second-order nonlinear optical effect [1]. No detailed data are available on the third-order nonlinear optical constants for group-IV semiconductor alloys.

11.5.2 III–V semiconductor alloy The second-order nonlinear optical susceptibilities for w-AlxGa1xN with 0 x 0.666 have been measured by Sanford et al. [25]. These authors determined the nonlinear optical susceptibility constants d31 and d33 at l ¼ 1.064 mm as a function of x under the assumption of d31 ¼ d15. These results are shown in Figure 11.3(a), together with the endpoint data taken from Adachi [1]. The nonlinear susceptibility constant d31 decreases almost linearly with increasing x, while d33 largely scatters. The nonlinear optical susceptibility d14 at l ¼ 1.064 mm in AlxGa1xAs has been measured using a reflected second harmonics method by Ohashi et al. [26]. They reported the magnitudes of d14 relative to GaAs over the whole alloy range 0 x 1.0. These results are shown in Figure 11.3(b). The GaAs and AlAs d14 values in Adachi [3] are in the ranges 119–170 and 32 pm/V, respectively.

15

1.0

140

10

-10 -15 (a) w-AlxGa1-xN

-20 -25

0

0.2 0.4 0.6 0.8 1.0 x

100 d14 (pm/V)

d33

|d14(x)/d14(GaAs)|

d31, d33 (pm/V)

0 -5

120

0.8

d31

5

0.6 0.4

80 60 40

0.2 0

(b) AlxGa1-xAs 0

0.2 0.4 0.6 0.8 1.0 x

(c) ZnxCd1-xTe

20 0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 11.3 Second-order nonlinear optical susceptibility constants dij in (a) w-AlxGa1xN, (b) AlxGa1xAs and (c) ZnxCd1xTe. The experimental data in (a) are taken from Adachi [1] and Sanford et al. [25], in (b) from Ohashi et al. [26] and in (c) from Adachi [4] (open circles) and Zappettini et al. [31] (solid circles)

362

PROPERTIES OF SEMICONDUCTOR ALLOYS

The third-order nonlinear susceptibility |x (3)| in GaxIn1xPyAs1y/InP (lg 1.5 mm) has been determined using a forward degenerate four-wave mixing method [27]. The |x (3)| value obtained was 3.8 103 esu. The two-photon absorption coefficient b has been discussed both theoretically and experimentally for non-alloyed group-IV, III–Vand II–VI semiconductors [1]. Krishnamurthy et al. [28] showed that theoretically, b can be increased or decreased by adding In or Al to the GaN compound. Experimentally, Villeneuve et al. [29] obtained the spectral dependence of b near half the band gap of Al0.18Ga0.82As. The b increased with decreasing wavelength l (0.05 cm/GW at l ¼ 1.65 mm and 1.2 cm/GW at l 1.49 cm/GW). The three-photon absorption coefficient a in Al0.18Ga0.82As was also measured for photon energies between onehalf and one-third the band gap by Kang et al. [30]. They found that a decreases with decreasing l from a 0.13 cm3/GW2 at l ¼ 1.66 mm to a 0.03 cm3/GW2 at l ¼ 1.50 mm.

11.5.3 II–VI semiconductor alloy The second harmonic generation efficiency has been examined in the near-IR region (l ¼ 1.5 and 1.9 mm) of ZnxCd1xTe with x ¼ 0, 0.1, 0.2 and 1.0 [31]. The d14 data for ZnxCd1xTe [31], together with the endpoint data taken from Adachi [4], have been plotted in Figure 11.3(c). The solid line represents the linear least-squares fit given by d14 ¼ 73 13x pm/V. The second-order nonlinear constant d14 of CdxHg1xTe with x ¼ 0.277 has been determined to be 350 40 pm/V [32]. The second harmonic generation has also been measured at l ¼ 1.06 mm as a function of x for w-ZnxCd1xS and w-CdSxSe1x [33]. The two-photon absorption phenomena have been studied in several II–VI semiconductor alloys [34,35]. The maximum value of the two-photon absorption coefficient b is observed for x ¼ 0.4 in c-MgxZn1xSe (0 x 0.4) [34]. In c-ZnxCd1xSe and w-ZnxCd1xSe (0 x 1.0), the reduction in the band gap is accompanied by a smooth rise of b [35]. Tunability of the twophoton absorption coefficient has also been demonstrated by adjusting the electrical field in a CdxHg1xTe photodiode with a cutoff wavelength of 5.2 mm [24].

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [3] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [4] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [5] S. A. Geidur, Opt. Spectrosc. 49, 105 (1980). [6] S. Adachi and K. Oe, J. Appl. Phys. 54, 6620 (1983). [7] S. M. Kikkarin, D. V. Petrov, A. V. Tsarev, and I. B. Yakovkin, Proc. SPIE 1932, 234 (1993). [8] P. Ziobrowski, M. Drozdowski, M. Szybowicz, F. Firszt, S. Ł e˛ gowski, and H. Meczy ˛ nska, J. Appl. Phys. 93, 3805 (2003). [9] S. Adachi and C. Hamaguchi, J. Phys. Soc. Jpn 44, 343 (1978). [10] X. Tang, K. G. Irvine, D. Zhang, and M. G. Spencer, Appl. Phys. Lett. 59, 1938 (1991). [11] R. A. Soref, J. Appl. Phys. 72, 626 (1992).

ELASTO-OPTIC, ELECTRO-OPTIC AND NONLINEAR OPTICAL PROPERTIES [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34] [35]

363

M. Glick, F.-K. Reinhart, and D. Martin, J. Appl. Phys. 63, 5877 (1988). H. G. Bach, J. Krauser, H. P. Nolting, R. A. Logan, and F. K. Reinhart, Appl. Phys. Lett. 42, 692 (1983). S. Adachi and K. Oe, J. Appl. Phys. 56, 74 (1984). A. Zappettini, L. Cerati, A. Milani, S. M. Pietralunga, P. Boffi, and M. Martinelli, J. Electron. Mater. 30, 743 (2001). L. Baldassarre, A. Cingolani, and M. Sibilano, Opt. Commun. 26, 72 (1978). S. Bini and C. Razzetti, Phys. Status Solidi A 148, 603 (1995). S. Adachi and K. Oe, J. Appl. Phys. 56, 1499 (1984). R. G. Verenchikova and A. O. Konstantinov, Sov. Phys. Semicond. 18, 242 (1984). R. H. Kingston, Appl. Phys. Lett. 34, 744 (1979). K. Okamoto, S. Matsuoka, Y. Nishiwaki, and K. Yoshida, J. Appl. Phys. 56, 2595 (1984). B. Kn€upfer, P. Kiesel, A. H€ofler, P. Riel, G. H. D€ohler, and E. Veuhoff, Appl. Phys. Lett. 62, 2072 (1993). L. Samuel, Y. Brada, and R. Beserman, Phys. Rev. B 37, 4671 (1988). H. Y. Cui, Z. F. Li, Z. L. Liu, C. Wang, X. S. Chen, X. N. Hu, Z. H. Ye, and W. Lu, Appl Phys. Lett. 92, 021128 (2008). N. A. Sanford, A. V. Davydov, D. V. Tsvetkov, A. V. Dmitriev, S. Keller, U. K. Mishra, S. P. DenBaars, S. S. Park, J. Y. Han, and R. J. Molnar, J. Appl. Phys. 97, 053512 (2005). M. Ohashi, T. Kondo, R. Ito, S. Fukatsu, Y. Shiraki, K. Kumata, and S. S. Kano, J. Appl. Phys. 74, 596 (1993). M. N. Islam, E. P. Ippen, E. G. Burkhardt, and T. J. Bridges, J. Appl. Phys. 59, 2619 (1986). S. Krishnamurthy, K. Nashold, and A. Sher, Appl. Phys. Lett. 77, 355 (2000). A. Villeneuve, C. C. Yang, G. I. Stegeman, C.-H. Lin, and H.-H. Lin, Appl. Phys. Lett. 62, 2465 (1993). J. U. Kang, A. Villeneuve, M. Sheik-Bahae, G. I. Stegeman, K. Al-hemyari, J. S. Aitchison, and C. N. Ironside, Appl. Phys. Lett. 65, 147 (1994). A. Zappettini, S. M. Pietralunga, A. Milani, D. Piccinin, M. Fere, and M. Martinelli, J. Electron. Mater. 30, 738 (2001). A. W. Wark, D. Pugh, L. E. A. Berlouis, and F. R. Cruickshank, J. Appl. Phys. 89, 306 (2001). R. A. Soref and H. W. Moos, J. Appl. Phys. 35, 2152 (1964). B. Derkowska, B. Sahraoui, X. N. Phu, G. Glowacki, and W. Bala, Opt. Mater. 15, 199 (2000). M. S. Brodin and D. B. Goer, Sov. Phys. Semicond. 5, 219 (1971).

12 Carrier Transport Properties 12.1 INTRODUCTORY REMARKS The electrical resistivity r, together with the thermal resistivity W, for CuxAu1x is shown in Figure 12.1. The solid and open circles correspond to the ordered (CuAu and Cu3Au) and disordered alloys, respectively. The experimental data are taken from various sources. The W data plots in Figure 12.1(b) are the same as those in Figure 2.24. The solid and dashed lines in Figure 12.1(a) are calculated from Equation (A.17) with CCuAu ¼ 60 mW cm and with and without properly taking into account the effect of alloy ordering at x ¼ 0.5 and 0.75 (CuAu and Cu3Au), respectively. As mentioned in Section 2.5.1, the Wiedemann–Franz law states that the ratio of the thermal conductivity K (¼W1) to the electrical conductivity s (¼r1) is proportional to the temperature. Thus, at any temperature s (r) is proportional to K (W), as can be seen in Figure 12.1. In semiconductor alloys, the potential fluctuations of electrons are a result of the compositional disorder. This effect produces a peculiar scattering mechanism, namely, alloy scattering. Alloy-scattering-limited mobility is represented as [1] mal e

pﬃﬃﬃﬃﬃﬃ 2p e h4 Nal ¼ 3 ðkTÞ1=2 ðme Þ5=2 xð1xÞðDUe Þ2

ð12:1Þ

where me is the electron effective mass, Nal is the density of alloy sites, DUe is the alloy scattering potential and x and (1 x) are the mole fractions of the endpoint materials. The alloy scattering mechanism shown in Equation (12.1) leads to a decrease in the electron mobility me at x „ 0 or 1.0. Not only the electrons but also the holes are subject to potential fluctuations as a result of the compositional disorder. Alloy scattering may, therefore, be observable both in n- and p-type 5=2 semiconductor alloys. However, because of its mass dependence (i.e. me;h ), the scattering strength may be weaker in p-type alloys than in n-types. The electron and hole Hall mobilities (me and mh) measured at room temperature for a number of non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Table 12.1. These values, together with the bowing parameters ce and ch listed in Table 12.2, can be used for obtaining the mobilities of alloys of arbitrary composition. Electron and hole saturation drift velocities, minority carrier lifetimes and impact ionization coefficients for some non-alloyed group-IV, III–V and II–VI semiconductors can be found in Adachi [2].

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

366

PROPERTIES OF SEMICONDUCTOR ALLOYS 20

3 (a)

(b)

CuxAu1-x

W (cmK/W)

ρ (μΩ cm)

15

10

2

1

5 CuAu Cu3Au

0 0

0.2 0.4 0.6 0.8 1.0 x

CuAu Cu3Au

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.1 Electrical r and thermal resistivities W for CuxAu1x at 300 K. The theoretical curves are obtained from Equation (A.17) (Equation (2.25)) with CCuAu ¼ 60 mW cm (r) and 8.15 cm K/W (W) and with (solid lines) and without properly taking into account the alloy ordering effect at x ¼ 0.5 and 0.75 (CuAu and Cu3Au) (dashed lines), respectively

Table 12.1 Room-temperature electron and hole Hall mobilities me and mh for some cubic and hexagonal semiconductors. d ¼ diamond, zb ¼ zinc-blende, h ¼ hexagonal, w ¼ wurtzite, rs ¼ rocksalt System Material IV

III–V

a

me (cm2/V s) mh (cm2/V s) System Material

Diamond (d) Si (d) Ge (d) 3C-SiC (zb) 6H-SiC (h) BP (zb) AlN (w) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

2800 1750a 4330 980 375 190 125 80 294 200 760 1245 189 9340 12040 3100 6460 33000 77000

Drift (conductivity) mobility

1500 480 2400 60 100 500 14 450 105 420 350 370 140 450 1000 39 180 450 1100

II–VI MgO (rs) ZnO (w) ZnS (zb) ZnS (w) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdS (w) CdSe (w) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

me (cm2/V s) mh (cm2/V s) 440 275 140 1500 600 216 85 390 900 1260a 230 22000 32000

10 267 72 355 100 48 50 104 320

CARRIER TRANSPORT PROPERTIES

367

Table 12.2 Bowing parameters ce and ch for the electron and hole mobilities me and mh in some group-IV binaries, and III–V and II–VI ternaries System IV III–V

Alloy CxSi1x SixGe1x w-AlxGa1xN GaxIn1xP AlxGa1xAs AlxIn1xAs GaxIn1xAs AlxGa1xSb GaxIn1xSb GaPxSb1x GaAsxSb1x InPxAs1x InPxSb1x InAsxSb1x

ce (cm2/V s) ch (cm2/V s) System 5200 11000 900 18000 35000 26000 42000 20000 30000 110000 30000

3600 2200

IIVI

40 520

Alloy CdxHg1xSe ZnxCd1xTe c-ZnSxSe1x ZnSexTe1x

ce (cm2/V s) ch (cm2/V s) 30000 2800 3200

160

600 2500 1000 2500

12.2 LOW-FIELD MOBILITY 12.2.1 Group-IV Semiconductor Alloy (a) CSi binary alloy The electron and hole mobilities me and mh for Si (x ¼ 0), diamond (x ¼ 1.0) and 3C-SiC (x ¼ 0.5), respectively are shown in Figure 12.2(a). The solid lines represent the quadratic fits of Equation (A.17) with ce,h in Table 12.2. Note that 3C-SiC is an ordered form of CxSi1x, or in other words, a compound. We can, thus, expect no alloy scattering in 3C-SiC. However, the 3CSiC mobilities are smaller than the mean values of diamond and Si, especially for mh. The lower 3C-SiC values may be due to its poorer crystalline quality. (b) SiGe binary alloy Figure 12.2(b) shows the electron and hole mobilities me and mh for SixGe1x. It is obvious that not only is alloy scattering, but also that the other scattering mechanisms and the effective masses modified through the change of the band structure influence the electron mobility in this alloy. The mass and temperature dependence of each scattering mechanism 5=2 is summarized in Table 12.2 of Adachi [2], including alloy scattering (m / me;h , m/T1/2). The most prominent example is the decrease in me at x 0.15, which corresponds to the transition from a Ge-like CB (L) to a Si-like CB (X or D) (Figure 6.8). The main effect on me is, thus, associated with the increase in the electron conductivity mass in the Si-like CB for x 0.15 (Figure 7.3). For SixGe1x, mh was not found to be strongly dependent on x.

368

PROPERTIES OF SEMICONDUCTOR ALLOYS

μe (103 cm2/Vs)

5 4

5

(a) Cx Si1-x

Ge-like CB

3

3 3C-SiC

2

2

1

1

0

0

2.0

μh (103 cm2/Vs)

(b) SixGe1-x

4

1.5

3.0

(a) CxSi1-x

2.0

1.0

1.5 1.0

3C-SiC

0.5 0 0

(b) SixGe1-x

2.5

0.5 0.2

0.4

0.6

0.8

1.0

0 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 12.2 Electron and hole mobilities me and mh for (a) CxSi1x and (b) SixGe1x at 300 K. The solid lines show the calculated results using Equation (A.17) and the numeric parameters in Tables 12.1 and 12.2

12.2.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N alloy The electron mobility me for some (III, III)–V ternary alloys, w-AlxGa1xN, w-AlxIn1xN and w-GaxIn1xN, plotted against x is shown in Figure 12.3. The me values for w-AlxGa1xN can be expressed by Equation (A.5) with ce ¼ 900 cm2/V s (Table 12.2). No large me values have been obtained for w-AlxIn1xN and w-GaxIn1xN ternaries. Very weak temperature dependence of 1.5

4 (a) w-AlxGa1-xN

μe (103 cm2/Vs)

1.2

4 (b) w-AlxIn1-xN

1.0 (c) w-GaxIn1-xN

3

3

2

2

0.9

0.6

0.6

0.4 1

0.3 0

(d) AlxGa0.98-xIn0.02N

0.8

0 0.2 0.4 0.6 0.8 1.0 x

0

1

0 0.2 0.4 0.6 0.8 1.0 x

0

0.2

0 0.2 0.4 0.6 0.8 1.0 x

0 0 0.2 0.4 0.6 0.8 1.0 x

Figure 12.3 Electron mobility me for (a) w-AlxGa1xN, (b) w-AlxIn1xN, (c) w-GaxIn1xN and (d) w-AlxGa0.98xIn0.02N at 300 K. The solid line in (a) shows the result calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

CARRIER TRANSPORT PROPERTIES

369

the free-electron density in w-GaxIn1xN with In-rich compositions (x 0.08) [3] suggests that the materials are metallic-like. (b) (III, III)–P alloy The electron and hole mobilities for GaxIn1xP are shown in Figure 12.4. Some data correspond to those for GaxIn1xP lattice-matched to GaAs. The lowest CB in InP (x ¼ 0) is located at the G point, while that in GaP is at the X point. The large (small) me value for InP (GaP) is principally due to the small (large) electron effective mass in the G (X) valley, as shown in Figure 12.4(a) by the open circles. There is a clear relationship between the electron effective mass mac (or mGe ) and electron mobility me. We can estimate from Equations (12.19) and (12.21) in Adachi [2] the X- and G-valley electron mobilities to be 220 (InP) and 990 cm2/V s (GaP), respectively. These values are plotted in Figure 12.4(a) by the open triangles. 8

2.5 (a)

(b)

2.0 Γ-valley

μh (102 cm2/Vs)

μe (103 cm2/Vs)

6

4

2 X-valley

0 0

0.2 0.4 0.6 0.8 1.0 x

1.5 1.0 0.5 0 0

GaxIn1-xP 0.2 0.4 0.6 0.8 1.0 x

Figure 12.4 Electron and hole mobilities me and mh for GaxIn1xP at 300 K. The solid line in (b) shows the result calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

(c) (III, III)–As alloy The electron and hole mobilities for some (III, III)As ternaries are plotted in Figure 12.5. The AlxGa1xAs and AlxIn1xAs ternaries show the G X crossover at x 0.4 and 0.6, respectively (Figures 6.20 and 6.22). These alloys may, thus, provide an abrupt change in me at such crossover points due to the different effective masses at the G and X valleys. From Equations (12.19) and (12.21) in Adachi [2], we can estimate the X- and G-valley electron mobilities to be 330 (GaAs) and 830 cm2/V s (AlAs), respectively. These values are also shown in Figure 12.5(a) by the open triangles. Similarly, we can estimate the X-valley electron mobility to be 270 cm2/V s, as plotted in Figure 12.5(b) by the open triangle (InAs). The G-electron bowing parameters for me and those for mh are listed in Table 12.2. The low-field transport properties of AlxGa1xAs have also been reviewed in more detail in Adachi [1]. (d) (III, III)–Sb alloy The electron and hole mobilities for some (III, III)–Sb ternaries are plotted in Figure 12.6. Like (Al, III)–As in Figure 12.5, the AlxGa1xSb and AlxIn1xSb alloys show the G X crossover at

370

PROPERTIES OF SEMICONDUCTOR ALLOYS

μh (102 cm2/Vs)

μe (104 cm2/Vs)

1.2

4

4

(a) AlxGa1-xAs

(b) AlxIn1-xAs

0.9

(c) GaxIn1-xAs

3 Γ-valley

0.6

Γ-valley

2

0.3

2

1

X-valley

0

0

5

5

(a) AlxGa1-xAs

4

3

1

X-valley

0 5

(b) AlxIn1-xAs

4

3

3

3

2

2

2

1

1

1

0

0

0.2

0.4

0.6

0.8

1.0

0

0

0.2

0.4

x

0.6

(c) GaxIn1-xAs

4

0.8

0 1.0 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 12.5 Electron and hole mobilities me and mh for (a) AlxGa1xAs, (b) AlxIn1xAs and (c) GaxIn1xAs at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

μh (103 cm2/Vs)

μe (104 cm2/Vs)

2.0

10

(a) AlxGa1-xSb 1.5 Γ-valley

1.0

8

10

(b) AlxIn1-xSb Γ-valley

6

6

4

4

0.5

2

2

0 1.5

0

0

1.5

2.0

X-valley

(a) Al xGa1-xSb

(c) Ga xIn1-xSb

8

(b) AlxIn1-xSb

1.0

1.0

0.5

0.5

(c) GaxIn1-xSb 1.5 1.0

0

0

0.2

0.4

0.6 x

0.8

1.0 0 0

0.5 0.2

0.4

0.6 x

0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 12.6 Electron and hole mobilities me and mh for (a) AlxGa1xSb, (b) AlxIn1xSb and (c) GaxIn1xSb at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

x 0.5 and 0.7, respectively (Figures 6.25 and 6.26). We can, thus, expect an abrupt change in me at such crossover points, although no enough experimental data are available. The dependence of me on x in GaxIn1xSb can be successfully explained using ce ¼ 42000 cm2/ V s (Table 12.2).

CARRIER TRANSPORT PROPERTIES

371

(e) Dilute-nitride III–(V, V) alloy The electron mobility should be lower in dilute-nitride III–V alloys due to strong carrier scattering and enhanced electron effective masses [4,5]. The experimental mobility me for dilutenitrideGaNxAs1x andInNxAs1x ternariesisshowninFigure12.7.Itcanbeseenthattheaddition of small concentrations of N to GaAs or InAs leads to a large reduction in me. The reduction in me determined experimentally seemed to be larger than that predicted theoretically [4,5]. 105

105

(b) InNxAs1-x

104

μe (cm2/Vs)

μe (cm2/Vs)

(a) GaN xAs1-x

103

102 0

1

2 3 x (at%)

4

104

103

102 0

1

2 3 x (at%)

4

Figure 12.7 Electron mobility me for (a) dilute-nitride GaNxAs1x and (b) dilute-nitride InNxAs1x at 300 K. The open circles show the endpoint binary data taken from Table 12.1

Since the VB of the III–V semiconductors is mainly characterized by the electron orbital of the group V anions [2], we can expect that N addition will not have a strong effect on the hole mobility. However, the experimental mh value dramatically decreased from 300 cm2/V s at x ¼ 0 at% (GaAs) to 80 cm2/V s at x ¼ 1 at% [6]. This drop in mh is likely correlated with the increase in crystalline defects introduced by nitrogen doping. (f) Ga–(V, V) alloy Figure 12.8 shows the electron and hole mobilities for some Ga–(V, V) ternary alloys. As in AlxGa1xAs, the CB in GaPxAs1x shows the G X crossover at x ¼ 0.48 (Figures 6.33). GaPxAs1x, thus, shows an abrupt change in me near x ¼ 0.48. The open triangles in Figures 12.8 (a) and 12.8(b) plot the X- and G-valley electron mobilities for GaAs (GaSb) and GaP as estimated from Equations (12.19) and (12.21) in Adachi [2], respectively. (g) In–(V, V) alloy The experimental electron mobility for some In–(V, V) ternaries have been plotted in Figure 12.9. The solid lines represent the me versus x curves calculated from Equation (A.5) with ce taken from Table 12.2.

12.2.3 III–V Semiconductor Quaternary Alloy (a) Dilute-nitride alloy The free-electron concentration and mobility have been found to be significantly reduced by the incorporation of N into Si-doped dilute-nitride GaxIn1xNyP1y [7] and GaxIn1xNyAs1y [8,9].

372

PROPERTIES OF SEMICONDUCTOR ALLOYS

μe (103 cm2/Vs)

10

15

(a) GaPxAs1-x

8

12

Γ-valley

6

15

(b) GaPxSb1-x

9

4 X-valley

6 Γ-valley

3

0

X-valley

3

0

1.2

0

1.2

1.2

(a) GaPxAs1-x

(b) GaPxSb1-x

(c) GaAsxSb1-x

0.9

0.9

0.9

0.6

0.6

0.6

0.3

0.3

0.3

0

0

0.2

0.4

0.6

0.8

(c) GaAsxSb1-x

9

6

2

μh (103 cm2/Vs)

12

0 1.0 0

0.2

x

0.4

0.6

0.8

0 1.0 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 12.8 Electron and hole mobilities me and mh for (a) GaPxAs1x, (b) GaPxSb1x and (c) GaAsxSb1x at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

4

10

10

(a) InPx As1-x

μ e (10 4 cm 2 /Vs)

3

(b) InPx Sb1-x

(c) InAsx Sb1-x

8

8

6

6

4

4

2

2

2

1

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.9 Electron mobility me for (a) InPxAs1x, (b) InPxSb1x and (c) InAsxSb1x at 300 K. The solid lines show the results calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

No significant effect of N incorporation has, however, been observed on the hole transport properties of Be-doped GaxIn1xNyAs1y [9] and Zn-doped GaNxAs1xSb1xy [10]. (b) (III, III)–(V, V) alloy The variation in me and mh with y for GaxIn1xPyAs1y/InP is shown in Figure 12.10. The solid lines represent the quadratic expressions given by (in cm2/V s)

CARRIER TRANSPORT PROPERTIES 1.8

2.5

(a)

(b)

1.5

2.0

1.2

μ h (10 2 cm2 /Vs)

μ e (10 4 cm2 /V s)

GaxIn1-xPyAs1-y/InP

0.9 0.6

1.5

1.0

0.5

0.3 0

373

0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

0.4

y

0.6

0.8

1.0

y

Figure 12.10 Electron and hole mobilities me and mh for GaxIn1xPyAs1y/InP at 300 K. The solid lines show the results calculated using Equation (12.2)

me ðyÞ ¼ 1520030740y þ 22000y2

ð12:2aÞ

mh ðyÞ ¼ 183383y þ 380y2

ð12:2bÞ

As can be seen in Figure 12.10, alloy scattering produces a mobility minimum at y 0.7 and 0.5 for me and mh, respectively. The low-field transport properties of GaxIn1xPyAs1y/InP have also been reviewed in more detail in Adachi [11]. (c) (III, III, III)–V alloy The electron mobility me versus x for w-AlxGa0.98xIn0.02N [12] has been plotted in Figure 12.3(d). As in w-AlxGa1xN (Figure 12.3(a)), me for w-AlxGa0.98xIn0.02N greatly decreases with increasing x. The electron mobility me as a function of x for (AlxGa1x)0.53In0.47P/GaAs and (AlxGa1x)0.48In0.52As/InP is plotted in Figures 12.11(a) and 12.11(b), respectively. The solid lines in Figures 12.11(a) and 12.11(b) show, respectively, the quadratic expressions given by (in cm2/V s) me ðxÞ ¼ 43006000x þ 3000x2

ð12:3aÞ

me ðxÞ ¼ 1520038400x þ 32000x2

ð12:3bÞ

The experimental data in Figure 12.11(a) are taken from Sotoodeh et al. [13] (open circle) and Hofmann et al. [14] (solid circles). The CB in (AlxGa1x)0.53In0.47P/GaAs shows the G X crossover at x 0.64 (Figure 6.49). Thus, the experimental me data for x > 0.64 in Figure 12.11 (a) seem to be questionably large.

374

PROPERTIES OF SEMICONDUCTOR ALLOYS 6

2.0

(a)

(b)

4 X-valley

3 2

(AlxGa1-x)0.48In0.52As/InP

1.5

μe (104 cm2/Vs)

μe (103 cm2/Vs)

5 (Al Ga ) In P/GaAs x 1-x 0.53 0.47

1.0

0.5

Γ-valley

1 0

0

0.2

0.4

0.6

0.8

0 0

1.0

x

0.2

0.4

0.6

0.8

1.0

x

Figure 12.11 Electron mobility me for (a) (AlxGa1x)0.53In0.47P/GaAs and (b) (AlxGa1x)0.48In0.52As/ InP at 300 K. The solid lines show the calculated results using Equation (12.3)

12.2.4 II–VI Semiconductor Alloy (a) (II, II)–O ternary alloy The large band-gap alloy MgxZn1xO is the subject of growing interest in connection with the development of UV optoelectronic devices based on ZnO. The low-field hole mobility mh is plotted against x for MgxZn1xO in Figure 12.12(a). The x ¼ 0.2 data provides the highest alloy mh value of 6.42 cm2/V s [15]. 103

2.5

(a) Mgx Zn1-xO

μh(cm /Vs) 2

mixed phase wurtzite rocksalt

100

10-1 0

μe (104 cm2/Vs)

2.0

102

101

(b) Cdx Hg1-xSe

1.5 1.0

zinc-blende wurtzite mixed phase

0.5

0.2 0.4 0.6 0.8 1.0 x

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.12 Electron mobility me for (a) MgxZn1xO and (b) CdxHg1xSe at 300 K. The solid line in (b) shows the results calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

(b) (II, II)–Se ternary alloy The electron Hall mobility for Bridgman-grown MgxZn1xSe (x 0.07) and MgxCd1xSe (x 0.4) has been measured at T ¼ 11300 K [16]. The me values for MgxZn1xSe

CARRIER TRANSPORT PROPERTIES

375

(MgxCd1xSe) with x ¼ 0.07 (0.4) are 225 (100) and 20 (0.2) cm2/V s at 300 and 11 K, respectively. The very low me values observed at low temperatures were considered to be due to the conduction at the impurity band. The electron mobility me for Bridgman-grown Fe-doped ZnxHg1xSe with x 0.072 has been measured in the temperature range 1.7–300 K [17]. The electron mobility for CdxHg1xSe has also been measured by several authors. The experimental data for CdxHg1xSe are shown in Figure 12.12(b). The solid line represents the dependence of me on x using Equation (A.5) with the numeric parameters shown in Tables 12.1 and 12.2. (c) (II, II)–Te ternary alloy Figure 12.13 shows the electron Hall mobility me for some (II, II)–Te ternaries. The hole Hall mobility mh for ZnxCd1xTe is also plotted in the lower part of Figure 12.13. Because ZnxCd1xTe is one of the most promising materials for use in room-temperature nuclear detectors, the carrier drift mobilities were usually measured in conjunction with the value of the mt (drift mobility–lifetime) product. Note that the solid triangles (me) in Figure 12.13(b) correspond to the electron drift mobility, not the Hall mobility. The highest me value for CdTe (x ¼ 0) reported so far is 1260 cm2/V s [18], which is considerably smaller than that predicted from the dashed line in Figure 12.13(b) (1600 cm2/V s).

μe (103 cm2/Vs)

1.2 0.9

3

(b) Zn xCd1-xTe 2

40 30

1

0.3

0.4

0.6

10 0.8

0

1.0 0 1.2

μh (102 cm2/Vs)

x

(c) Cd x Hg1-xTe

20

Γ-valley

0.2

semimetal

50

Hall mobility Drift mobility

X-valley

0.6

0 0

60

(a) Mg xCd1-xTe

0.2

0.4

0.6

0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

(b) ZnxCd1-xTe

0.9 0.6 0.3 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 12.13 Electron and hole Hall mobilities me and mh for (a) MgxCd1xTe, (b) ZnxCd1xTe and (c) CdxHg1xTe at 300 K. The electron drift mobilities are also shown by the solid triangles in (b). The solid line in (b) shows the result calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

As seen in Figure 12.13(c), the electron Hall mobility for CdxHg1xTe increases monotonically from x ¼ 0 to a peak at the semiconductorsemimetal transition x 0.08 with a peak mobility of 44000 cm2/V s and then drops monotonically with further increase in x. The lowfield electron and hole transport properties of CdxHg1xTe have been reviewed in more detail in Miles [19].

376

PROPERTIES OF SEMICONDUCTOR ALLOYS

(d) Zn–(V, V) ternary alloy The electronHall mobility forc-ZnSxSe1x and ZnSexTe1x ternaries is shown in Figures 12.14(a) and 12.14(b), respectively. The limited data predict that these alloys have considerably large bowing parameters ce, as listed in Table 12.2. 1.8

1.8

(b) ZnSe xTe1-x

1.5

1.5

1.2

1.2

μe (103 cm2/Vs)

μe (103 cm2/Vs)

(a) c-ZnS xSe1-x

0.9 0.6 0.3 0

0.9 0.6 0.3

0

0.2 0.4 0.6 0.8 1.0 x

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.14 Electron mobility me for (a) c-ZnSxSe1x and (b) ZnSexTe1x at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

12.3 HIGH-FIELD TRANSPORT 12.3.1 Group-IV Semiconductor Alloy No detailed studies concerning the high-field transport properties of group-IV semiconductor alloys have been reported.

12.3.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N alloy The high-field transport phenomena in AlxGa1xN and GaxIn1xN have been investigated using Monte Carlo simulation [20,21]. The electron drift velocity–field (ve E) characteristics obtained from these studies are summarized in Figure 12.15. The electron velocity at high fields tends to level off and is defined as the saturation velocity ve,sat. (b) (III, III)–P alloy The high-field transport properties of Ga0.5In0.5P/GaAs have been studied by several authors. Sakamoto et al. [22] determined the ve E curve for E up to 20 kV/cm at 300 K. Yee et al. [23] reported the temperature-dependent ve,sat up to 200 C by analyzing Ga0.5In0.5P/GaAs HBT characteristics. These results are shown in Figure 12.16. The electron drift velocity peaks at E 15 kV/cm with a value of vp 1.0 107 cm/s.

CARRIER TRANSPORT PROPERTIES

377

v Ep vp vsat 3.0

E

6 (a)

1.8 (b)

(c)

5 Ep (105 V/cm)

2.0

1.5

1.0 0

ve, sat (107 cm/s)

1.6

vp (107 cm/s)

2.5 4 3

1.4

2

1.2

AlxGa1-xN GaxIn1-xN

1

0.2 0.4 0.6 0.8 1.0 x

0 0

0.2 0.4 0.6 0.8 1.0 x

1.0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.15 (a) Peak electron drift velocity vp, (b) peak field Ep and (c) electron saturation velocity ve,sat for AlxGa1xN and GaxIn1xN obtained using the Monte Carlo simulation at 300 K

12

6

ve, sat (106 cm/s)

10 ve (106 cm/s)

Ga0.5In0.5P/GaAs

(a)

8 6 4

5 4 3

2 0

(b) 0

5

10 15 E (kV/cm)

20

2

0

50 100 150 200 250 T (°C)

Figure 12.16 (a) Electron drift velocity versus field curve and (b) electron saturation velocity as a function of temperature for Ga0.5In0.5P/GaAs at 300 K. The experimental data in (a) are taken from Sakamoto et al. [22] and in (b) from Yee et al. [23]

(c) (III, III)–As alloy The veE curves for AlxGa1xAs have been determined using a pump-probe technique and transferred-electron devices [24]. As can be seen in Figure 12.17(a), the electron drift velocity at any fixed field decreases with increasing x. The hole drift velocity versus field (vh E) curves for Al0.45Ga0.55As have also been studied using an ensemble Monte Carlo technique [25]. These results, together with the experimental vh E curve for GaAs, are shown in the lower part of Figure 12.17(a).

378

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 12.17 Electron and hole velocities versus filed curves for (a) AlxGa1xAs and (b) GaxIn1xAs. The data plotted in (a) are taken from Bhattacharya et al. [24] (ve E) and Brennan and Hess [25] (vh E, Monte Carlo simulation) and in (b) from Balynas et al. [26] (ve E) and Adachi [11] (vh E)

Figure 12.17(b) plots the ve,h E curves for Ga0.47In0.53As/InP [11,26]. We also show in the lower part of Figure 12.17(b) the experimental and calculated vh E curves for GaAs and InP, respectively. The hole velocity saturation in these materials occurs at fields of about 100 kV/cm, which are much higher than those for the electrons ( b [78,84]. The a and b coefficients for strained Ga0.2In0.8As have also been measured by fabricating lateral p-i-n diodes [85]. The results indicate that both a and b are larger than those for GaAs and furthermore b is larger than a. (d) (III, III)–Sb alloy Hildebrand et al. [86] reported resonance enhancement of b in a low field region for AlxGa1xSb with x ¼ 0.065 where E0 is equal to D0 (Figure 6.25). The b/a ratio exceeded 20. Zhingarev et al. [87] also measured a, b and their ratio for AlxGa1xSb (x ¼ 00.23). Kuwatsuka et al. [88] observed no strong enhancement of b/a in AlxGa1xSb near x ¼ 0.06. The b/a ratio obtained by Kuwatsuka et al. was 5 at the low electric field of 1.6 105 V/cm. More recently, Gouskov et al. [89] studied the impact ionization phenomena in AlxGa1xSb at x ¼ 0, 0.04 and 0.08 and obtained a maximum b/a at x ¼ 0.04. Theoretically, Rmou et al. [90] showed that if the alloy disorder in AlxGa1xSb is neglected, b exhibits a continuous variation with D0/E0; if not, b is strongly increased and shows a maximum at x ¼ 0.02. (e) Dilute-nitride III–(V, V) alloy A p-i-n avalanche photodiode using GaNxAs1x/GaAs was demonstrated [91]. The b/a ratio obtained was 0.4.

CARRIER TRANSPORT PROPERTIES

385

(f) Ga–(V, V) alloy The a and b values were determined for GaAsxSb1x (x ¼ 0.875 and 0.90) at 77 and 300 K [92]. The b/a ratios reported were 0.3 at 300 K (x ¼ 0.875), 0.4 at 77 K and 0.6 at 300 K (x ¼ 0.90). (g) In–(V, V) alloy The impact ionization coefficients for InAs0.12Sb0.88 were investigated and it was found that b is about 5 times larger than a in the field E ¼ (4 6) 104 V/cm [93].

12.5.3 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) alloy The a and b values at high electric fields ( > 180 kV/cm) for GaxIn1xPyAs1y/InP have been determined by Osaka et al. [94,95]. The b/a ratio versus y for GaxIn1xPyAs1y/InP [95] is reproduced in Figure 12.23. The ratio was found to increase with increasing y and to become unity, a ¼ b, at y 0.6. 101

β/α

GaxIn1-xPyAs1-y/InP 100

10-1 0

0.2

0.4

0.6

0.8

1.0

y

Figure 12.23 b/a ratio for GaxIn1xPyAs1y/InP. The experimental data are taken from Osaka et al. [95]

As in Ga0.47In0.53As, anomalous low-field behavior of a was observed in GaxIn1xPyAs1y/ InP [96]. No anomaly for b was observed in this quaternary [97]. The impact ionization phenomena in Ga0.80In0.20As0.17Sb0.83/GaSb have been studied by fabricating mesa photodiodes [98]. The a and b values in Equation (12.4) have been determined to be A ¼ 2.41 106 cm1 and B ¼ 4.45 105 V/cm with m ¼ 2.0 (a) and A ¼ 1.98 106 cm1 and B ¼ 3.69 105 V/cm with m ¼ 2.0 (b), respectively. The resulting b/a ratio is 47. (b) (III, III, III)–V alloy The parameterized a and b values in Equation (12.4) have been determined for Al0.24Ga0.24 In0.53As/InP to be A ¼ 2.29 107 cm1 and B ¼ 3.59 106 V/cm with m ¼ 1.0 (a) and A ¼ 1.42 107 cm1 and B ¼ 3.73 106 V/cm with m ¼ 1.0 (b), respectively (E ¼ 400–500 kV/cm) [99]. The relationship a > b can be predicted from these parameters. The impact ionization coefficients a and b for a strained Al0.22Ga0.63In0.15As layer grown on Al0.3Ga0.7 As/GaAs by MBE have also been determined by fabricating lateral p-i-n diodes [85].

386

PROPERTIES OF SEMICONDUCTOR ALLOYS

12.5.4 II–VI Semiconductor Alloy Although Brennan and Mansour [100] calculated the electron impact ionization coefficient for CdxHg1xTe, no detailed experimental data are available for II–VI semiconductor alloys.

REFERENCES [1] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [2] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [3] S. -K. Lin, K. -T. Wu, C. -P. Huang, C. -T. Liang, Y. H. Chang, Y. F. Chen, P. H. Chang, N. C. Chen, C. A. Chang, H. C. Peng, C. F. Shih, K. S. Liu, and T. Y. Lin, J. Appl. Phys. 97, 046101 (2005). [4] M. P. Vaughan and B. K. Ridley, Phys. Rev. B 72, 075211 (2005). [5] S. Fahy, A. Lindsay, H. Ouerdane, E. P. OReilly, Phys. Rev. B 74, 035203 (2006). [6] A. J. Ptak, S. W. Johnston, S. Kurtz, D. J. Friedman, and W. K. Metzger, J. Cryst. Growth 251, 392 (2003). [7] Y. G. Hong, A. Nishikawa, and C. W. Tu, Appl. Phys. Lett. 83, 5446 (2003). [8] Y. -S. Kang, L. H. Robins, A. G. Birdwell, A. J. Shapiro, W. R. Thurber, M. D. Vaudin, M. M. E. Fahmi, D. Bryson, and S. N. Mohammad, J. Appl. Phys. 98, 093714 (2005). [9] N. Miyashita, Y. Shimizu, and Y. Okada, J. Appl. Phys. 102, 044904 (2007). [10] G. M. Peake, K. E. Waldrip, T. W. Hargett, N. A. Modine, and D. K. Serkland, J. Cryst. Growth 261, 398 (2004). [11] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons Ltd, New York, 1992. [12] Y. Liu, H. Jiang, T. Egawa, B. Zhang, and H. Ishikawa, J. Appl. Phys. 99, 123702 (2006). [13] M. Sotoodeh, A. H. Khalid, and A. A. Rezazadeh, J. Appl. Phys. 87, 2890 (2000). [14] T. Hofmann, G. Leibiger, V. Gottschalch, I. Pietzonka, and M. Schubert, Phys. Rev. B 64, 155206 (2001). [15] Z. P. Wei, B. Yao, Z. Z. Zhang, Y. M. Lu, D. Z. Shen, B. H. Li, X. H. Wang, J. Y. Zhang, D. X. Zhao, X. W. Fan, and Z. K. Tang, Appl. Phys. Lett. 89, 102104 (2006). [16] K. Perzynska, F. Firszt, S. Ł e˛ gowski, H. Meczy ˛ nska, J. Szatkowski, M. Biernacka, A. Gajlewicz, S. Tarasenko, and P. Zaleski, J. Cryst. Growth 214/215 904 (2000). [17] W. Dobrowolski, R. R. Gał˛a zka, E. Grodzicka, J. Kossut, and B. Witkowska, Phys. Rev. B 48, 17848 (1993). [18] J. C. Erickson, H. W. Yao, R. B. James, H. Hermon, and M. Greaves, J. Electron. Mater. 29, 699 (2000). [19] R. W. Miles, in Properties of Narrow Gap Cadmiun-based Compounds, EMIS Datareviews Series No. 10 (edited by P. Capper), INSPEC, London, 1994, p. 221. [20] A. F. M. Anwar, S. Wu, and R. T. Webster, IEEE Trans. Electron Dev. 48, 567 (2001). [21] E. Bellotti, F. Bertazzi, and M. Goano, J. Appl. Phys. 101, 123706 (2007). [22] R. Sakamoto, K. Nakata, and S. Nakajima, Physica B 272, 250 (1999). [23] M. Yee, P. A. Houston, and J. P. R. David, J. Appl. Phys. 91, 1601 (2002). [24] P. K. Bhattacharya, U. Das, and M. J. Ludowise, Phys. Rev. B 29, 6623 (1984). [25] K. Brennan and K. Hess, J. Appl. Phys. 59, 964 (1986). [26] V. Balynas, A. Krotkus, A. Stalnionis, A. T. Gorelionok, N. M. Shmidt, and J. A. Tellefsen, Appl. Phys. A 51, 357 (1990). [27] D. Hahn and A. Schlachetzki, J. Electron. Mater. 21, 1147 (1992).

CARRIER TRANSPORT PROPERTIES

387

[28] A. Patane, A. Ignatov, D. Fowler, O. Makarovsky, L. Eaves, L. Geelhaar, and H. Riechert, Phys. Rev. B 72, 033312 (2005). [29] J. -S. Rieh, P. K. Bhattacharya, and E. T. Croke, IEEE Trans. Electron Dev. 47, 883 (2000). [30] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [31] S. Chakraborty, M. K. Bera, S. Bhattacharya, P. K. Bose, and C. K. Maiti, Thin Solid Films 504, 73 (2006). [32] A. G. Ulyashin, N. V. Abrosimov, A. Bentzen, A. Suphellen, E. Sauar, and B. G. Svensson, Mater. Sci. Semicond. Process. 9, 772 (2006). [33] R. Shivaram, G. Niu, J. D. Cressler, and E. T. Croke, Solid-State Electron. 44, 559 (2000). [34] S. K. Samanta, S. Maikap, S. Chatterjee, and C. K. Maiti, Solid-State Electron. 47, 893 (2003). [35] M. S. Carroll and C. A. King, J. Appl. Phys. 93, 1656 (2003). [36] I. Z. Mitrovic, O. Buiu, S. Hall, J. Zhang, Y. Wang, P. L. F. Hemment, H. A. W. El Mubarek, and P. Ashburn, Semicond. Sci. Technol. 20, 95 (2005). [37] A. Cremades, M. Albrecht, J. Krinke, R. Dimitrov, M. Stutzmann, and H. P. Strunk, J. Appl. Phys. 87, 2357 (2000). [38] K. Kumakura, T. Makimoto, N. Kobayashi, T. Hashizume, T. Fukui, and H. Hasegawa, J. Cryst. Growth 298, 787 (2007). [39] B. F. Levine, W. T. Tsang, C. G. Bethea, and F. Capasso, Appl. Phys. Lett. 41, 470 (1982). [40] B. F. Levine, C. G. Bethea, W. T. Tsang, F. Capasso, K. K. Thornber, R. C. Fulton, and D. A. Kleinman, Appl. Phys. Lett. 42, 769 (1983). [41] R. K. Ahrenkiel, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 221. [42] R. A. J. Thomeer, P. R. Hageman, and L. J. Giling, Appl. Phys. Lett. 64, 1561 (1994). [43] J. Degani, R. F. Leheny, R. E. Nahory, and J. P. Heritage, Appl. Phys. Lett. 39, 569 (1981). [44] P. Hill, J. Schlafer, W. Powazinik, E. Eichen, and R. Olshansky, Appl. Phys. Lett. 50, 1260 (1987). [45] N. Chand, in Properties of Lattice-matched and Strained Indium Gallium Arsenide, EMIS Datareviews Series No. 8 (edited by P. Bhattacharya), INSPEC, London, 1993, p. 127. [46] D. Vignaud, D. A. Yarekha, J. F. Lampin, M. Zaknoune, S. Godey, and F. Mollot, Appl. Phys. Lett. 90, 242104 (2007). [47] R. E. Welser, R. S. Setzko, K. S. Stevens, E. M. Rehder, C. R. Lutz, D. S. Hill, and P. J. Zampardi, J. Phys. Condens. Matter 16, S3373 (2004). [48] S. Sakai, M. Umeno, and Y. Amemiya, Jpn. J. Appl. Phys. 19, 109 (1980). [49] M. M. Tashima, L. W. Cook, and G. E. Stillman, J. Electron. Mater. 11, 831 (1982). [50] C. H. Henry, B. F. Levine, R. A. Logan, and C. G. Bethea, IEEE J. Quantum. Electron. QE-19, 905 (1983). [51] J. M. Borrego, S. Saroop, R. J. Gutmann, G. W. Charache, T. Donovan, P. F. Baldasaro, and C. A. Wang, J. Appl. Phys. 89, 3753 (2001). [52] D. Donetsky, S. Anikeev, G. Belenky, S. Luryi, C. A. Wang, and G. Nichols, Appl. Phys. Lett. 81, 4769 (2002). [53] S. Anikeev, D. Donetsky, G. Belenky, S. Luryi, C. A. Wang, J. M. Borrego, and G. Nichols, Appl. Phys. Lett. 83, 3317 (2003). [54] C. A. Wang, D. A. Shiau, D. Donetsky, S. Anikeev, G. Belenky, and S. Luryi, Appl. Phys. Lett. 86, 101910 (2005). [55] T. N. Danilova, B. E. Zhurtanov, A. N. Imenkov, and Y. P. Yakovlev, Semicond. 39, 1235 (2005). [56] V. Bhagwat, Y. G. Xiao, I. Bhat, P. Dutta, T. F. Refaat, M. N. Abedin, and V. Kumar, J. Electron. Mater. 35, 1613 (2006). [57] S. A. Wood, C. H. Molloy, P. M. Smowton, P. Blood, and C. C. Button, IEEE J. Quantum Electron. 36, 742 (2000). [58] P. C. Mogensen, G. Jones, N. Cain, P. Blood, D. J. Mowbray, S. W. Bland, D. Peggs, and R. P. Petrie, Inst. Phys. Conf. Ser. 162, 161 (1999).

388

PROPERTIES OF SEMICONDUCTOR ALLOYS

[59] O. Lopatiuk, W. Burdett, L. Chernyak, K. P. Ip, Y. W. Heo, D. P. Norton, S. J. Pearton, B. Hertog, P. P. Chow, and A. Osinsky, Appl. Phys. Lett. 86, 012105 (2005). [60] P. Lemasson, A. Forveille-Boutry, and R. Triboulet, J. Appl. Phys. 55, 592 (1984). [61] J. Franc, P. H€oschl, E. Belas, R. Grill, P. Hlıdek, P. Moravec, and J. Bok, Nucl. Instrum. Methods Phys. Res. A 434, 146 (1999). [62] K. N. Oh, K. H. Kim, J. K. Hong, Y. C. Chung, S. U. Kim, and M. J. Park, J. Cryst. Growth 184, 1247 (1998). [63] P Capper, Y. Nemirovsky, R. Fastow, C. L. Jones, in Properties of Narrow Gap Cadmiun-based Compounds, EMIS Datareviews Series No. 10 (edited by P. Capper), INSPEC, London, 1994, pp. 227–241. [64] J. Lee, A. L. Gutierrez-Aitken, S. H. Li, and P. K. Bhattacharya, IEEE Trans. Electron Dev. 43, 977 (1996). [65] K. Yeom, J. M. Hinckley, and J. Singh, J. Appl. Phys. 80, 6773 (1996). [66] K. Kunihiro, K. Kasahara, Y. Takahashi, and Y. Ohno, IEEE Electron Dev. Lett. 20, 608 (1999). [67] T. Tut, M. Gokkavas, B. Butun, S. Butun, E. Ulker, and E. Ozbay, Appl. Phys. Lett. 89, 183524 (2006). [68] S. -L. Fu, T. P. Chin, M. C. Ho, C. W. Tu, and P. M. Asbeck, Appl. Phys. Lett. 66, 3507 (1995). [69] R. Ghin, J. P. R. David, S. A. Plimmer, M. Hopkinson, G. J. Rees, D. C. Herbert, and D. R. Wight, IEEE Trans. Electron Dev. 45, 2096 (1998). [70] C. K. Chia, J. P. R. David, G. J. Rees, S. A. Plimmer, R. Grey, and P. N. Robson, J. Appl. Phys. 84, 4363 (1998). [71] S. A. Plimmer, J. P. R. David, R. Grey, and G. J. Rees, IEEE Trans. Electron Dev. 47, 1089 (2000). [72] X. G. Zheng, P. Yuan, X. Sun, G. S. Kinsey, A. L. Holmes, B. G. Streetman, and J. C. Campbell, IEEE J. Quantum Electron. 36, 1168 (2000). [73] B. K. Ng, J. P. R. David, G. J. Rees, R. C. Tozer, M. Hopkinson, and R. J. Airey, IEEE Trans. Electron Dev. 49, 2349 (2002). [74] Y. L. Goh, A. R. J. Marshall, D. J. Massey, J. S. Ng, C. H. Tan, M. Hopkinson, J. P. R. David, S. K. Jones, C. C. Button, and S. M. Pinches, IEEE J. Quantum Electron. 43, 503 (2007). [75] D. Ritter, R. A. Hamm, A. Feygenson, and M. B. Panish, Appl. Phys. Lett. 60, 3150 (1992). [76] R. J. Malik, N. Chand, J. Nagle, R. W. Ryan, K. Alavi, and A. Y. Cho, IEEE Electron Dev. Lett. 13, 557 (1992). [77] A. Neviani, G. Meneghesso, E. Zanoni, M. Hafizi, and C. Canali, IEEE Electron Dev. Lett. 18, 619 (1997). [78] M. Yee, J. P. R. David, P. A. Houston, C. H. Tan, and A. Krysa, IEEE Trans. Electron Dev. 50, 2021 (2003). [79] W. K. Ng, C. H. Tan, J. P. R. David, P. A. Houston, M. Yee, and J. S. Ng, Appl. Phys. Lett. 83, 2820 (2003). [80] J. Bude and K. Hess, J. Appl. Phys. 72, 3554 (1992). [81] M. Isler, Phys. Rev. B 63, 115209 (2001). [82] C. H. Tan, G. J. Rees, P. A. Houston, J. S. Ng, W. K. Ng, and J. P. R. David, Appl. Phys. Lett. 84, 2322 (2004). [83] K. Y. Choo and D. S. Ong, J. Appl. Phys. 98, 023714 (2005). [84] J. S. Ng, C. H. Tan, J. P. R. David, G. Hill, and G. J. Rees, IEEE Trans. Electron Dev. 50, 901 (2003). [85] Y. C. Chen and P. K. Bhattacharya, J. Appl. Phys. 73, 465 (1993). [86] O. Hildebrand, W. Kuebart, and M. H. Pilkuhn, Appl. Phys. Lett. 37, 801 (1980). [87] M. Z. Zhingarev, V. I. Korolkov, M. P. Mikhailova, and V. V. Sazonov, Sov. Tech. Phys. Lett. 7, 637 (1981). [88] H. Kuwatsuka, T. Mikawa, S. Miura, N. Yasuoka, M. Ito, T. Tanahashi, and O. Wada, J. Appl. Phys. 70, 2169 (1991). [89] L. Gouskov, B. Orsal, M. Perotin, M. Karim, A. Sabir, P. Coudray, S. Kibeya, and H. Luquet, Appl. Phys. Lett. 60, 3030 (1992).

CARRIER TRANSPORT PROPERTIES

389

[90] A. Rmou, H. Luquet, L. Gouskov, M. Perotin, and P. Coudray, Jpn. J. Appl. Phys. 33, 4657 (1994). [91] G. S. Kinsey, D. W. Gotthold, A. L. Holmes, Jr., B. G. Streetman, and J. C. Campbell, Appl. Phys. Lett. 76, 2824 (2000). [92] V. M. Andreev, M. Z. Zhingarev, O. O. Iventeva, V. I. Korolkov, and M. P. Mikhaılova, Sov. Phys. Semicond. 15, 701 (1981). [93] B. A. Matveev, M. P. Mikhaılova, S. V. Slobodchikov, N. N. Smirnova, N. M. Stus, and G. N. Talalakin, Sov. Phys. Semicond. 13, 294 (1979). [94] F. Osaka, T. Mikawa, and T. Kaneda, Appl. Phys. Lett. 46, 1138 (1985). [95] F. Osaka, T. Mikawa, and T. Kaneda, IEEE J. Quantum Electron. QE-21, 1326 (1985). [96] N. Shamir and D. Ritter, IEEE Trans. Electron Dev. 47, 488 (2000). [97] N. Shamir and D. Ritter, IEEE Electron Dev. Lett. 21, 509 (2000). [98] I. A. Andreev, M. P. Mikhaılova, S. V. Melnikov, Y. P. Smorchkova, and Y. P. Yakovlev, Sov. Phys. Semicond. 25, 861 (1991). [99] M. Tsuji, K. Makita, I. Watanabe, and K. Taguchi, Appl. Phys. Lett. 65, 3248 (1994). [100] K. F. Brennan and N. S. Mansour, J. Appl. Phys. 69, 7844 (1991).

Index Page numbers in italic refer to figures or tables. Alloys are listed according to elemental composition. Abeles’s model 63–4 AlAsSb band-gap energies 174–5 optical properties 323 phonon frequencies 108 thermal conductivity 70 AlGaAs band offsets GaAs interface 278–9 GaInP interface 278 band-gap energies 157–60 deformation potential 263–4, 269–70, 271–2 effective masses 239–41 elastic properties 90, 96 electro-optic constant 358, 359 Franz–Keldysh effect 360 impact ionization coefficient 383 low-field mobility 369, 377–8 microhardness 93 minority-carrier transport 380–1 nonlinear optical constant 361–2 optical properties 316, 317 phonon frequencies 106–7, 113–15, 120 photoelastic constant 357, 358 piezoelectric constant 128–9 thermal conductivity 68, 69 thermal diffusivity 75–6 AlGaAsSb band offsets GaInAsSb interface 282 InP/InAs/GaSb interfaces 281 band-gap energies 187–8, 196 optical properties 328 Schottky barrier 296–7 AlGaIn and coherent epitaxy 37 phonon frequencies 108, 109

AlGaInAs band offsets, GaInAs interface 283 band-gap energies 194–5 effective masses 250, 251 impact ionization coefficient 385 optical properties 331–2 Schottky barrier 298–9 thermal conductivity 74 AlGaInN crystal lattice parameters 25, 26 low-field mobility 373–4 Schottky barrier 297–8 thermal conductivity 68, 69, 70 AlGaInP band offsets AlInP interface 282 GaInP interface 282–3 band-gap energies 187, 191, 193–4, 196 effective masses 250 elastic properties 81, 86 low-field mobility 373–4 minority-carrier transport 382 optical properties 330–1 Schottky barrier 298 thermal conductivity 74 AlGaN band offsets, GaN interface 283–4 band-gap energies 149–51 and critical thickness 38 deformation potential 261–2, 263 impact ionization coefficient 382 low-field mobility 368, 376, 377 minority-carrier transport 380 nonlinear optical constant 361 optical properties 311–12 phonon frequencies 105–6 piezoelectric constant 125 Schottky barrier 291

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

392

INDEX

AlGaNAs band-gap energies 184–5 optical properties 326–7 AlGaP band-gap energies 153, 154 effective masses 238–9 optical properties 314 AlGaPAs band-gap energies 186–7 optical properties 326–7 AlGaSb band-gap energies 163–5 effective masses 242–3 impact ionization coefficient 384 lattice parameters 26, 27 low-field mobility 369–70 Schottky barrier 294–5 AlInAs band offsets GaInAS interface 280 InP interface 279 band-gap energies 160–1 deformation potential 264 effective masses 240, 241 elastic properties 89, 90 optical properties 316–17, 318 Schottky barrier 293–4 AlInAsSb band offsets, GaInAsSb interface 282 band-gap energies 187, 188–9, 196 AlInN band offsets, GaN interface 284 band-gap energies 150, 152 low-field mobility 368–9 optical properties 313, 314 AlInP band offsets AlGaInP interface 282 GaInP interface 277–8 band-gap energies 153–5 deformation potential 262–3 effective masses 238–9, 240 optical properties 314–15 AlInSb band-gap energies 165–6 effective masses 242–3 low-field mobility 369–70 optical properties 319, 320 alloy scattering 365 alloys defined and described 1

AlPAs band-gap energies 174–5 effective masses 245 AlPSb band-gap energies 174–5 effective masses 245 optical properties 322 Au/GaInP rectifiers 292 band offsets see heterojunction band offsets band-gap energies background and theory bowing parameter 136 interpolation of parameters 4–7 ordered/disordered alloy 136–9 quasi-cubic band model 133–6, 135 group IV alloys binary 139–45 ternary 145–7, 149 III-V ternary alloys Al–(V, V) 174–5 Ga–(V, V) 175–9 In–(V, V) 179–84 dilute-nitride III–(V, V) 166–74 (III, III)–As 157–63 (III, III)–N 149–53 (III, III)–P 153–7 (III, III)–Sb 163–6 summary 183–4 III–V quaternary alloys dilute-nitride 184–93 (III, III, III)–V 193–5 III–(V, V, V) 195 summary 196–7 II–VI ternary alloys Cd–(VI, VI) 210–12 Zn–(VI, VI) 208–10 (II, II)–O 197–8 (II, II)–S 198–201 (II, II)–Se 201–4 (II, II)–Te 204–8 summary 214–16 II–VI quaternary alloys (II, II, II)–VI 213–14 (II, II)–(VI, VI) 212–13 summary 214–16 BeCdSe band-gap energies 199, 201, 202 optical properties 335 BeCdTe, band-gap energies 199, 201, 202 BeMgCdSe, band-gap energies 213–14

INDEX BeMgZnSe band offsets, ZnSe interface 289 band-gap energies 213, 214 optical properties 346 BeS/BeSe/BeTe, elastic properties 90–1, 93–4 BeZnCdSe, optical properties 346 BeZnO band-gap energies 197, 198, 199, 215 optical properties 332 BeZnSe band offsets, ZnSe interface 287–8 band-gap energies 199, 201–2 elastic properties 84–5, 86, 94 optical properties 335, 336 phonon frequencies 111, 118 photoelastic constant 357 BeZnTe band-energies 199, 201–2, 215 band-gap energies 199, 204–5 optical properties 339 phonon frequencies 111 bilayer model 34–5 binary mixed valence compounds 2–4 bond distances 21 bowing parameters 5, 6, 7, 136 dilute-nitride III–V alloys 167 electron and hole mobilities 367 III–V ternaries 184 II–VI ternaries 215 Brillouin scattering 357 carrier transport properties 365–7 high-field mobility 376–9 impact ionization coefficient 382–6 low-field mobility 367–76 minority-carrier transport 379–82 CdHgS, band-gap energies 199, 200–1 CdHgSe band-gap energies 199, 201, 203–4, 215 low-field mobility 374 optical properties 338–9 CdHgTe band offsets, CdTe interface 288–9 band-gap energies 199, 208, 215 Debye temperature 58–9 effective masses 252, 254 Frank–Keldysh effect 361 impact ionization coefficient 386 low-field mobility 375 minority-carrier transport 382 nonlinear optical constant 362

393

optical properties 342 phonon frequencies 109, 111 specific heat 56 thermal conductivity 74–5 thermal expansion coefficient 63 CdSeTe band-gap energies 211–12 optical properties 346 phase diagram 50 CdSSe band-gap energies 210–11 effective masses 253 electro-optic constant 359–60 Franz–Keldysh effect 360–1 optical properties 344–5 CdSTe band-gap energies 211 lattice parameters 31 optical properties 345 phase diagram 49–50 CGe band-gap energies 140–1, 147, 149 optical properties 309 chalcopyrite structures 14 cleavage plane 41 coherent epitaxy bilayer model 32–3 critical thickness 37–9 elastic strain and lattice deformation 33–7 lattice-mismatch of dilute-nitrides 167–8 compliance constants 81, 82–3 composite structures see coherent epitaxy compound semiconductors 1, 10 conduction band structure 133, 134 critical thickness 37–9 crystal density calculation 22 data 18, 19 crystal structure 2 lattice constant/parameters 15–31 random alloy 11 spontaneous ordering 11–15 CSi band offsets Si interface 276–7 SiGe interface 277 band-gap energies 139–40, 147–9 Debye temperature 57–8 effective masses 234–7 elastic properties 89 electro-optic constant 358

394

INDEX

CSi (Continued) Fr€ohlich coupling constant 130 lattice mismatch in epilayers 35–6 low-field mobility 367 microhardness 92 optical properties 308–9 piezoelectric constant 125, 127 thermal conductivity 66, 67 thermal diffusivity 75–6 CSiGe band offsets, Si interface 276–7 band-gap energies 145–7 minority-carrier transport 380 optical properties 311 Schottky barrier 291 CuAu elastic properties 82 electrical resistivity 365, 366 lattice constant 15–16 thermal resistivity 65–6, 365, 366 CuAu-I structure 12, 14, 15, 66 CuPt-B structure 12, 14, 15 energy-band diagram 136, 137 Debye temperature 52–3, 56–7 group IV alloy 57–8 III–V alloy 58 II–VI alloy 58–9 deformation potential (intervalley) group IV alloy 270–1 III–V alloy 271–2 deformation potential (intravalley) group IV alloy 259–61 high-symmetry points 267–9 III–V ternary alloy 261–6 high-symmetry points 269–70 III–V quaternary alloy 266 II–VI quaternary alloy 266–7 deformation potential (phonon) 121–3 density-of-state effective mass 229, 232 diamond structure 21 dielectric constants 308 dispersion 307 drift velocities 365 effective masses background and theory compositional dependence 254 electron effective mass 229–30, 231 hole effective mass 230–2, 233, 234, 235, 236

interpolation scheme 232–4 temperature and pressure dependence 254–6 group IV binary alloys 234–8 III–V ternary alloys Al–(V, V) 245, 246 Ga–(V, V) 245–6 In–(V, V) 246–7 dilute-nitride III–(V, V) 243–5 (III, III)–As 239–42 (III, III)–N 238, 239 (III, III)–P 238–9 (III, III)–Sb 242–3 III–V quaternary alloys dilute-nitride 248 (III, III, III)–V 250–1 (III, III)–(V, V) 248–50 II–VI ternary alloys (II, II)–VI 251–3 II–(VI, VI) 253 II–VI quaternary alloys (II, II)–(VI, VI) 253–4 elastic constants 81, 82–3 group IV alloy 81 III–V alloy 81, 83–4 II–VI 84–6 pressure effect 88 and sound velocity 96–7 temperature effect 86–8 third-order constant 39 see also Young’s modulus elastic strain 33–7 elasto-optic effect 357–8 electrical resistivity 365, 366 electro-optic constants linear 358–60 quadratic 360–1 electron mobility See low-field mobility; minority-carrier transport elemental semiconductors 1, 2 energy-band structure see band-gap energies; effective masses epitaxy see coherent epitaxy Franz–Keldysh effect 360–1 Fr€ ohlich coupling constant 129–31 GaAsIn, phase diagram 46, 47 GaAsInP specific heat 55 thermal conductivity and diffusivity 75–6

INDEX GaAsSb band-gap energies 178–9 effective masses 246 impact ionization coefficient 385 optical properties 324 phonon frequencies 100, 108 Schottky barrier 295–6 thermal conductivity 73 GaInAs band offsets AlGaInAs interface 283 AlInAS interface 280 GaAs interface 284–6 GaN interface 284 InP interface 279–80 band-gap energies 161, 163 deformation potential 265 effective masses 240, 241–2, 256 elastic properties 89, 90 impact ionization coefficient 383–4 low-field mobility 377–8 near neighbour distances 28 optical properties 318–19 phase diagram 46, 47 piezoelectric constant 128 Schottky barrier 294 thermal conductivity 68, 69, 70 GaInAsSb band offsets AlGaAsSb interface 282 AlInAsSb interface 282 GaSb/InP/InAs interfaces 281 band-gap energies 196 effective masses 249–50 optical properties 328–30 Schottky barrier 296–7 thermal conductivity 70, 71, 72 GaInN band offsets, GaN interface 284 band-gap energies 150, 151, 152–3 and critical thickness 38 deformation potential 262, 263 low-field mobility 368, 376, 377 near neighbour distances 28, 29 optical properties 313–14 phase diagram 47–8 phonon frequencies 105–6 piezoelectric constant 126–8 thermal conductivity 68, 69, 70 GaInNAs band offsets, GaAs interface 286–7

band-gap energies 166–7, 168, 185 effective masses 248, 254, 256 optical properties 326 GaInNP band-gap energies 185 optical properties 326 GaInP band offsets AlGaInP interface 282–3 AlInP interface 277–8 GaAs interface 277 band-gap energies 137–9, 155–7 deformation potential 263 effective masses 239, 240 elastic properties 89, 90 Franz–Keldysh effect 360 impact ionization coefficient 383 low-field mobility 369 nonlinear optical constant 362 optical properties 315–16 phonon frequencies 100, 108, 115 photoelastic constant 357 Schottky barrier 292 thermal conductivity 73 GaInPAs band offsets, InP interface 280–1 band-gap energies 187, 189–91, 196–7 and coherent epitaxy 34–5, 38 deformation potential 266, 267 effective masses 248–9, 256 elastic properties 81, 86, 87, 88, 96 Fr€ ohlich coupling constant 131 impact ionization coefficient 385 low-field mobility 372–3, 378–9 microhardness 92–3, 94 minority-carrier transport 381–2 near neighbour distances 28, 29 phonon frequencies 108 piezoelectric constant 128–9 Schottky barrier 296 thermal conductivity 70, 71, 72 GaInPSb, minority-carrier transport 381–2 GaInSb band-gap energies 166, 167, 168 effective masses 242–3 elastic properties 81, 83, 85 microhardness 93 minority-carrier transport 381 optical properties 319, 320 phase diagram 46, 47 phase transition 40–1

395

396

INDEX

GaInSb (Continued) phonon frequencies 107, 108 Schottky barrier 294–5 thermal conductivity 68, 69, 70 GaNAs band offsets, GaAs interface 286 band-gap energies 166–7, 168, 171–2 and coherent epitaxy 36 deformation potential 265–6 effective masses 243–4 impact ionization coefficient 384 low-field mobility 371, 378 mode Gr€uneisen parameter 121 optical properties 321, 322 GaNAsSb, band offsets, GaAs interface 287 GaNP effective masses 243 optical properties 320–1 GaNP, band-gap energies 170–1 GaNPAs, band-gap energies 185–6 GaNSb band-gap energies 172 optical properties 321 GaPAs band-gap energies 175–6 deformation potentials 263–4, 266, 269–70 effective masses 245, 246 low-field mobility 371, 372 optical properties 323–4 phonon frequencies 108, 115, 116, 122–3 GaPSb band-gap energies 176–7 optical properties 324 Schottky barrier 295 GaSbAs, low-field mobility 371, 372 GeSn band-gap energies 144–5, 147, 148 optical properties 309–10 Grimm–Sommerfeld rule 2–4 Gr€uneisen parameter 119–21 phonon deformation potential 121–3 Hall mobilities 366, 367 heterojunction band offsets 275 group IV systems 275–7 III–V lattice matched system ternary alloy 277–80 quaternary alloy 280–3 III–V lattice mis-matched system II–V systems 287–9

283–7

HgSeTe, phase diagram 51 high-field transport group IV 376 III–V ternary alloys dilute-nitride III–(V, V) 378 (III, III)–As 377–8 (III, III)–N 376 (III, III)–P 376–7 III–V quaternary alloys 378–9 II–IV alloys 379 high-frequency dielectric constant 308 hole effective mass 230–2, 233, 234, 235, 236 hole mobilities 366, 367 impact ionization coefficient group IV alloys 382 III–V ternary alloys dilute-nitride III–(V, V) 384–5 Ga–(V, V) 385 In–(V, V) 385 (III, III)–As 383–4 (III, III)–N 382–3 (III, III)–P 383 (III, III)–Sb 384 III–V quaternary alloys (III, III, III)–V 385 (III, III)–(V, V) 385 II–VI 386 InAsSb band offsets, GaSb interface 280 band-gap energies 181–3 effective masses 247 impact ionization coefficient 385 low-field mobility 371, 372 optical properties 325 InGaAs, Fr€ ohlich coupling 129 InNAs band-gap energies 173 effective masses 244–5 low-field mobility 371 InNP band-gap energies 173 optical properties 322 InNSb band-gap energies 174 effective masses 245 InPAs band-gap energies 179, 180 Debye temperature 58 effective masses 246–7, 255, 256

INDEX low-field mobility 371, 372 optical properties 324–5 specific heat 54, 55 thermal conductivity 70, 71 InPAsSb band-gap energies 195, 196 effective masses 250–1 InPSb band-gap energies 179–81 low-field mobility 371, 372 optical properties 325 interpolation schemes band-gap 4–7 effective masses 232–4 intravalley/intervalley deformation potential see deformation potential ionicity 9, 10 isotopic abundance 9 lattice constants/parameters Cu–Au alloy 15–16 group IV semiconductor 19–22 III–V semiconductor 22–9 II–VI semiconductor 29–31 non-alloyed semiconductors 16–19 lattice strain/deformation/mismatch see coherent epitaxy lattice-matching data 22, 23, 24, 30 linear electro-optic constant 358–60 long-wavelength phonon see phonon low-field mobility 366, 367 group IV binary alloys 367–8 III–V ternary alloys dilute-nitride III–(V, V) 370 Ga–(V, V) 371 In–(V, V) 371 (III–III)–As 369 (III–III)–N 368–9 (III–III)–P 369 (III–III)–Sb 369–70 III–V quaternary alloys dilute-nitride 371–2 (III, III, III)–V 373–4 (III, III)–(V, V) 372–3 II–VI ternary alloys Zn–(V, V) 375 (II, II)–O 374 (II, II)–Se 374–5 (II, II)–Te 375 Luttinger’s parameters 231, 233, 234

Matthews–Blakeslee theory 38 melting points 51, 52–3 see also phase diagrams MgCdSe band-gap energies 199, 201, 202–3, 215 low-field mobility 374–5 optical properties 337 MgCdTe band-gap energies 199, 206, 215 optical properties 340 MgZnCdSe band offsets, ZnCdSe interface 289 band-gap energies 214 optical properties 346–7 MgZnO band offsets, CdS interface 287 band-gap energies 197–8, 199, 215 and coherent epitaxy 37 deformation potential 267 effective masses 251–2 low-field mobility 374 minority-carrier transport 382 optical properties 332–3 phase diagram 48–9 MgZnS band-gap energies 198–9, 205 optical properties 333–4 MgZnSe band offsets ZnCdSe interface 289 ZnSe interface 287–8 band-gap energies 199, 201, 202, 215 low-field mobility 374–5 nonlinear optical constant 362 optical properties 335–7 thermal expansion coefficient 63 MgZnSeTe optical properties 346 phonon frequencies 112 MgZnSSe band offsets, ZnSe interface 289 bang-gap energies 212–13 effective masses 253–4 optical properties 346 phonon frequencies 111–12 MgZnSTe, band-gap energies 212, 213 MgZnTe band-gap energies 199, 205–6, 215 optical properties 339–40 Schottky barrier 299

397

398

INDEX

microhardness group IV alloy 92 III–V alloy 92–3 II–VI alloy 93–6 minority–carrier transport group IV alloys binary 379–80 ternary 380 III–V ternary alloys (III, III)–Ga 381 (III, III)–N 380 III–V quaternary alloys (III, III, III)–V 382 (III, III)–(V, V) 381–2 II–IV alloys 382 mode Gr€uneisen see Gr€uneisen parameter molecular weight calculating 9–10 non-alloyed semiconductor data 18, 19 multilayer structures see coherent epitaxy nonlinear optical constant

361–2

optical properties dielectric constants 308 dispersion relations 307 group IV alloys binary 308–11 ternary 311 III–V ternary alloys Al–(V, V) 322–3 Ga–(V, V) 323–4 In–(V, V) 324–6 dilute-nitride III–(V, V) 320–2 (III, III)–As 316–20 (III, III)–N 311–14 (III, III)–P 314–16 III–V quaternary alloys dilute-nitride 326 (III, III, III)–V 330–2 (III, III)–(V, V) 326–30 III–(V, V, V) 332 II–VI ternary alloys Cd–(VI, VI) 344–6 Zn–(VI, VI) 343–4 (II, II)–O 332–3 (II, II)–S 333–5 (II, II)–Se 335–9 (II, II)–Te 339–42 II–VI quaternary alloys (II, II, II )–VI 346–7

(II, II)–(VI, VI) 346 see also elasto-optic; electro-optic ordering see spontaneous ordering periodic table 2 phase diagrams group IV alloys 45 III–V alloys 45–8 II–VI alloys 48–51 phase transition, structural 39–41 Phillips ionicity 9, 10 phonon frequencies/modes 99–100, 101, 102, 104–5, 110 group IV alloy 100–4, 112–13 III–V alloy 104–9, 113–15 II–VI alloy 109–12, 115–19 mode Gr€ uneisen parameter 119–21 phonon deformation potential 121–3 temperature and pressure dependence 112–19 photoelastic coefficient 357–8 piezoelectric semiconductors 97, 126 stress and strain constants 125–9 pseudomorphic epitaxy 37–9 quadratic electro-optic constant

360–1

reflectivity 307 refractive index 307 resistivity electrical 365, 366 thermal 64, 65, 67, 68, 365, 366 Schottky barrier 289–90 group IV alloys 290–1 III–V ternary alloys Ga–(V, V) 295–6 (III, III)–As 292–4 (III, III)–N 291 (III, III)–P 292 (III, III)–Sb 294–5 III–V quaternary alloys (III, III, III)–V 297–9 (III, III)–(V, V) 296–7 II–VI ternary alloys Zn–(VI, VI) 300 (II, II)–Te 299 semiconductor types 1 SiC 1, 2 Franz–Keldysh effect 360 phonon frequencies 100, 102

INDEX SiGe band offsets, Si interface 276 band-gap energies 148 relaxed alloy 141–3 strained alloy 143–4 and critical thickness 38, 39 crystal lattice parameters 19–22 deformation potential 259–61, 269 effective masses 237–8 elastic properties 81, 84, 85 electro-optic constant 358 Fr€ohlich coupling constant 130 impact ionization coefficient 382, 383 low-field mobility 367–8 minority-carrier transport 379–80 optical properties 309–10 ordered structures 12, 13–14 phase diagram 45, 46 phonon frequencies 100–4, 113, 121–2 Schottky barrier 290–1 specific heat 53–4 thermal conductivity 66, 68 SiGeSn, band gap energies 147 SiSn, band gap energies 148–9 sound velocity 96–7 specific heat group IV alloys 51, 52–3, 53–4 III–V alloys 54–5 II–VI alloys 55 spontaneous ordering energy-band gaps 136–9 group IV alloy 11, 12 III-V alloy 12, 14–15 II–VI alloy 12, 15 structural phase transition 39–41 surface energy 41 tetrahedral rule 3–4 thermal conductivity 52–3, 63–6, 67 group IV alloy 66–8 III–V alloy 68–74 II–VI alloy 74–5 thermal diffusivity 75–6 thermal expansion coefficient 52–3 group IV alloys 59–61 III–V alloys 61–3 II–VI alloys 63 thermal resistivity 64, 65, 67, 68, 365, 366 thin films see critical thickness transport see carrier transport

399

valence band structure 133, 134 valence binary compounds 3–4 valence electrons 2–3 Varshni parameters 159–60, 163 Vegard law 20, 25–6, 28, 36, 37, 57, 141 Wiedemann–Franz law 65, 365 wurtxite structure 21 Young’s modulus group IV alloy 89 III–V alloy 89–90 II–VI alloy 90–2 zinc blende structure 21 energy band diagram 136, 137 ZnCdO band-gap energies 198, 199, 215 optical properties 333 ZnCdS band offsets, ZnS interface 287 band-gap energies 199, 200, 215 deformation potential 267 nonlinear optical constant 362 optical properties 334–5 phase transition 40, 41 phonon frequencies 109, 111 ZnCdSe band offsets MgSSe interface 289 MgZnCdSe interface 289 MgZnSe interface 289 ZnSe interface 287–8 band-gap energies 199, 201, 203, 215 elastic properties 91–2 Franz–Keldysh effect 360–1 nonlinear optical constant 362 optical properties 337–8 phase transition 40, 41 phonon frequencies 109–11, 115–16, 118 ZnCdSSe, band offsets, ZnSSe interface 289 ZnCdTe band offsets CdTe interface 288 ZnTe interface 288 deformation potential 266–7 elastic properties 85, 87, 88 electro-optic constant 358–60 lattice parameters 29, 30, 31 phase diagram 49 low-field mobility 375

400

INDEX

ZnCdTe (Continued) nonlinear optical constant 361, 362 optical properties 340–1 phonon frequencies 109–11 photoelastic constant 357 Schottky barrier 299 structural phase transition 39, 40 ZnHgS, band-gap energies 199, 200, 215 ZnHgTe band-gap energies 199, 207–8 effective masses 252–3 microhardness 94–5 minority-carrier transport 382 optical properties 342 phonon frequencies 109 thermal conductivity 74 thermal expansion coefficient 63 ZnOS band-gap energies 208–9 optical properties 343

ZnOSe band-gap energies 209 deformation potential 267 ZnSeTe band-gap energies 209, 210 elastic properties 91–2, 94 low-field mobility 376 optical properties 344 phonon frequencies 118 ZnSSe band offsets, ZnSe/ZnCdSe interfaces band-gap energies 209–10 deformation potential 267 low-field mobility 376 optical properties 343 Schottky barrier 300 thermal expansion coefficient 63 ZnSTe band-gap energies 209, 210 deformation potential 267 optical properties 343–4

289

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

Wiley Series in Materials for Electronic & Optoelectronic Applications Series Editors Peter Capper, SELEX Sensors and Airborne Systems Infrared Ltd, Southampton, UK Safa Kasap, University of Saskatchewan, Canada Arthur Willoughby, University of Southampton, Southampton, UK Published titles Bulk Crystal Growth of Electronic, Optical and Optoelectronic Materials, Edited by P. Capper Properties of Group-IV, III–V and II–VI Semiconductors, S. Adachi Charge Transport in Disordered Solids with Applications in Electronics, Edited by S. Baranovski Optical Properties of Condensed Matter and Applications, Edited by J. Singh Thin Film Solar Cells: Fabrication, Characterization and Applications, Edited by J. Poortmans and V. Arkhipov Dielectric Films for Advanced Microelectronics, Edited by M. R. Baklanov, M. Green and K. Maex Liquid Phase Epitaxy of Electronic, Optical and Optoelectronic Materials, Edited by P. Capper and M. Mauk Molecular Electronics: From Principles to Practice, M. Petty Luminescent Materials and Applications, Edited by A. Kitai CVD Diamond for Electronic Devices and Sensors, Edited by R. S. Sussman Forthcoming Titles Zinc Oxide Materials for Electronic and Optoelectronic Device Applications, Edited by C. Litton, D. C. Reynolds and T. C. Collins Mercury Cadmium Telluride: Growth, Properties and Applications, Edited by P. Capper and J. Garland Photovoltaic Materials: From Crystalline Silicon to Third-Generation Approaches, Edited by G. J. Conibeer Silicon Photonics: Fundamentals and Devices, J. Deen and P. K. Basu Inorganic Glasses for Photonics: Fundamentsls, Engineering and Applications, A. Jha, R. M. Almeida, M. Clara Goncalves and P. G. Kazansky

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors

SADAO ADACHI Gunma University, Gunma, Japan

This edition first published 2009 # 2009 John Wiley & Sons Ltd Registered office John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester, West Sussex, PO19 8SQ, United Kingdom For details of our global editorial offices, for customer services and for information about how to apply for permission to reuse the copyright material in this book please see our website at www.wiley.com. The right of the authors to be identified as the authors of this work has been asserted in accordance with the Copyright, Designs and Patents Act 1988. All rights reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted, in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, except as permitted by the UK Copyright, Designs and Patents Act 1988, without the prior permission of the publisher. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. Designations used by companies to distinguish their products are often claimed as trademarks. All brand names and product names used in this book are trade names, service marks, trademarks or registered trademarks of their respective owners. The publisher is not associated with any product or vendor mentioned in this book. This publication is designed to provide accurate and authoritative information in regard to the subject matter covered. It is sold on the understanding that the publisher is not engaged in rendering professional services. If professional advice or other expert assistance is required, the services of a competent professional should be sought. The publisher and the author make no representations or warranties with respect to the accuracy or completeness of the contents of this work and specifically disclaim all warranties, including without limitation any implied warranties of fitness for a particular purpose. This work is sold with the understanding that the publisher is not engaged in rendering professional services. The advice and strategies contained herein may not be suitable for every situation. In view of ongoing research, equipment modifications, changes in governmental regulations and the constant flow of information relating to the use of experimental reagents, equipment and devices, the reader is urged to review and evaluate the information provided in the package insert or instructions for each chemical, piece of equipment, reagent or device for, among other things, any changes in the instructions or indication of usage and for added warnings and precautions. The fact that an organization or Website is referred to in this work as a citation and/ or a potential source of further information does not mean that the author or the publisher endorses the information the organization or Website may provide or recommendations it may make. Further, readers should be aware that Internet Websites listed in this work may have changed or disappeared between when this work was written and when it is read. No warranty may be created or extended by any promotional statements for this work. Neither the publisher nor the author shall be liable for any damages arising herefrom. Library of Congress Cataloging-in-Publication Data Adachi, Sadao, 1950– Properties of semiconductor alloys : group-IV, III–V and II–VI semiconductors / Sadao Adachi. p. cm. Includes bibliographical references and index. ISBN 978-0-470-74369-0 1. Semiconductors–Materials. 2. Semiconductors–Analysis. 3. Silicon alloys. I. Title. TK7871.85.A32 2009 2008046980 621.38150 2–dc22 A catalogue record for this book is available from the British Library. ISBN 978-0-470-74369-0 (HB) Typeset in 10/12pt Times by Thomson Digital, Noida, India. Printed and bound in Great Britain by CPI Antony Rowe, Ltd, Chippenham, Wiltshire Front cover image of a photodiode array reproduced by kind permission of Dr. Jian-young Wu. Courtesy of Wutech Instruments and RedShirtImaging.

Contents Series Preface

xvii

Preface

xix

Abbreviations and Acronyms

xxi

Introductory Remarks A.1 An Alloy and a Compound A.2 Grimm–Sommerfeld Rule A.3 An Interpolation Scheme References 1 Structural Properties 1.1 Ionicity 1.2 Elemental Isotopic Abundance and Molecular Weight 1.3 Crystal Structure 1.3.1 Random Alloy 1.3.2 Spontaneous Ordering (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 1.4 Lattice Constant and Related Parameters 1.4.1 CuAu Alloy: Ordered and Disordered States 1.4.2 Non-alloyed Semiconductor 1.4.3 Semiconductor Alloy (a) Group-IV Semiconductor (b) III–V Semiconductor (c) II–VI Semiconductor 1.5 Coherent Epitaxy and Strain Problem 1.5.1 Bilayer Model 1.5.2 Elastic Strain and Lattice Deformation 1.5.3 Critical Thickness 1.6 Structural Phase Transition 1.7 Cleavage Plane 1.7.1 Cleavage 1.7.2 Surface Energy References

1 1 2 4 7 9 9 9 11 11 11 11 14 15 15 15 16 19 19 22 29 32 32 33 37 39 41 41 41 42

vi

CONTENTS

2 Thermal Properties 2.1 Melting Point and Related Parameters 2.1.1 Phase Diagram (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 2.1.2 Melting Point 2.2 Specific Heat 2.2.1 Group-IV Semiconductor Alloy 2.2.2 III–V Semiconductor Alloy 2.2.3 II–VI Semiconductor Alloy 2.3 Debye Temperature 2.3.1 General Considerations 2.3.2 Group-IV Semiconductor Alloy 2.3.3 III–V Semiconductor Alloy 2.3.4 II–VI Semiconductor Alloy 2.4 Thermal Expansion Coefficient 2.4.1 Group-IV Semiconductor Alloy 2.4.2 III–V Semiconductor Alloy 2.4.3 II–VI Semiconductor Alloy 2.5 Thermal Conductivity and Diffusivity 2.5.1 Thermal Conductivity (a) General Considerations (b) Group-IV Semiconductor Alloy (c) III–V Semiconductor Alloy (d) II–VI Semiconductor Alloy 2.5.2 Thermal Diffusivity (a) General Considerations (b) Alloy Value References

45 45 45 45 45 48 51 51 51 54 56 56 56 57 58 58 59 59 61 63 63 63 63 66 68 74 75 75 75 76

3 Elastic Properties 3.1 Elastic Constant 3.1.1 General Considerations 3.1.2 Room-temperature Value (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 3.1.3 External Perturbation Effect (a) Temperature Effect (b) Pressure Effect 3.2 Third-order Elastic Constant 3.3 Young’s Modulus, Poisson’s Ratio and Similar Properties 3.3.1 Group-IV Semiconductor Alloy 3.3.2 III–V Semiconductor Alloy 3.3.3 II–VI Semiconductor Alloy

81 81 81 81 81 81 84 86 86 88 89 89 89 89 90

CONTENTS

3.4

Microhardness 3.4.1 Group-IV Semiconductor Alloy 3.4.2 III–V Semiconductor Alloy 3.4.3 II–VI Semiconductor Alloy 3.5 Sound Velocity References

vii

92 92 92 93 96 97

4 Lattice Dynamic Properties 4.1 Phonon Dispersion Relationships 4.2 Phonon Frequency 4.2.1 General Considerations 4.2.2 Room-temperature Value (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 4.2.3 External Perturbation Effect (a) Group-IV Semiconductor Alloy (b) III–V Semiconductor Alloy (c) II–VI Semiconductor Alloy 4.3 Mode Gr€ uneisen Parameter 4.3.1 Phonon Deformation Potential References

99 99 99 99 100 100 104 109 112 112 113 115 119 121 123

5 Collective Effects and Some Response Characteristics 5.1 Piezoelectric Constant 5.1.1 General Considerations 5.1.2 Alloy Value 5.2 Fr€ ohlich Coupling Constant 5.2.1 General Considerations 5.2.2 Alloy Value References

125 125 125 125 129 129 129 131

6 Energy-band Structure: Energy-band Gaps 6.1 Introductory Remarks 6.1.1 Quasi-cubic Band Model 6.1.2 Bowing Parameter 6.1.3 Ordered Alloy 6.2 Group-IV Semiconductor Alloy 6.2.1 Binary Alloy (a) CSi (b) CGe (c) SiGe (d) GeSn 6.2.2 Ternary Alloy (a) CSiGe (b) SiGeSn 6.2.3 Summary

133 133 133 136 136 139 139 139 140 141 144 145 145 147 147

viii

6.3

6.4

CONTENTS

III–V Semiconductor Ternary Alloy 6.3.1 (III, III)–N Alloy (a) c-AlGaN (b) w-AlGaN (c) c-AlInN (d) w-AlInN (e) c-GaInN (f) w-GaInN 6.3.2 (III, III)–P Alloy (a) AlGaP (b) AlInP (c) GaInP 6.3.3 (III, III)–As Alloy (a) AlGaAs (b) AlInAs (c) GaInAs 6.3.4 (III, III)–Sb Alloy (a) AlGaSb (b) AlInSb (c) GaInSb 6.3.5 Dilute-nitride III–(V, V) Alloy (a) General Considerations (b) GaNP (c) GaNAs (d) GaNSb (e) InNP (f) InNAs (g) InNSb 6.3.6 Al–(V, V) Alloy 6.3.7 Ga–(V, V) Alloy (a) GaPAs (b) GaPSb (c) GaAsSb 6.3.8 In–(V, V) Alloy (a) InPAs (b) InPSb (c) InAsSb 6.3.9 Summary III–V Semiconductor Quaternary Alloy 6.4.1 Dilute-nitride Quaternary Alloy (a) AlGaNAs (b) GaInNP (c) GaInNAs (d) GaNPAs 6.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs (b) AlGaAsSb

149 149 149 150 152 152 152 152 153 153 153 155 157 157 160 161 163 163 165 166 166 166 170 171 172 173 173 174 174 175 175 176 178 179 179 179 181 183 184 184 184 185 185 185 186 186 187

CONTENTS

6.4.3

6.5

6.4.4 6.4.5 II–VI 6.5.1

6.5.2

6.5.3

6.5.4

6.5.5

6.5.6

6.5.7

6.5.8

(c) AlInAsSb (d) GaInPAs (e) GaInAsSb (III, III, III)–V Alloy (a) AlGaInP (b) AlGaInAs III–(V, V, V) Alloy Summary Semiconductor Alloy (II, II)–O Ternary Alloy (a) BeZnO (b) MgZnO (c) ZnCdO (II, II)–S Ternary Alloy (a) MgZnS (b) ZnCdS (c) ZnHgS (d) CdHgS (II, II)–Se Ternary Alloy (a) BeZnSe (b) BeCdSe (c) MgZnSe (d) MgCdSe (e) ZnCdSe (f) CdHgSe (II, II)–Te Ternary Alloy (a) BeZnTe (b) MgZnTe (c) MgCdTe (d) ZnCdTe (e) ZnHgTe (f) CdHgTe Zn–(VI, VI) Ternary Alloy (a) ZnOS (b) ZnOSe (c) ZnSSe (d) ZnSTe (e) ZnSeTe Cd–(VI, VI) Ternary Alloy (a) CdSSe (b) CdSTe (c) CdSeTe (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe (b) MgZnSeTe (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe

ix

188 189 191 193 193 194 195 196 197 197 197 197 198 198 198 200 200 200 201 201 202 202 202 203 203 204 204 205 206 206 207 208 208 208 209 209 210 210 210 210 211 211 212 212 213 213 213

x

CONTENTS

(b) BeZnCdSe (c) MgZnCdSe Summary

213 214 214 216

7 Energy-band Structure: Effective Masses 7.1 Introductory Remarks 7.1.1 Electron Effective Mass 7.1.2 Hole Effective Mass 7.1.3 Interpolation Scheme 7.2 Group-IV Semiconductor Alloy 7.2.1 CSi Binary Alloy 7.2.2 SiGe Binary Alloy 7.3 III–V Semiconductor Ternary Alloy 7.3.1 (III, III)–N Alloy 7.3.2 (III, III)–P Alloy 7.3.3 (III, III)–As Alloy (a) AlGaAs (b) AlInAs (c) GaInAs 7.3.4 (III, III)–Sb Alloy 7.3.5 Dilute-nitride III–(V, V) Alloy (a) Ga–(N, V) Alloy (b) In–(N, V) Alloy 7.3.6 Al–(V, V) Alloy 7.3.7 Ga–(V, V) Alloy (a) GaPAs (b) GaAsSb 7.3.8 In–(V, V) Alloy (a) InPAs (b) InAsSb 7.4 III–V Semiconductor Quaternary Alloy 7.4.1 Dilute-nitride Quaternary Alloy 7.4.2 (III, III)–(V, V) Alloy (a) GaInPAs (b) GaInAsSb 7.4.3 (III, III, III)–V Alloy (a) AlGaInP (b) AlGaInAs 7.4.4 III–(V, V, V) Alloy 7.5 II–VI Semiconductor Alloy 7.5.1 (II, II)–VI Ternary Alloy 7.5.2 II–(VI, VI) Ternary Alloy 7.5.3 (II, II)–(VI, VI) Quaternary Alloy 7.6 Concluding Remarks 7.6.1 Composition Dependence 7.6.2 External Perturbation Effect References

229 229 229 230 232 234 234 237 238 238 238 239 239 241 241 242 243 243 244 245 245 245 246 246 246 247 248 248 248 248 249 250 250 250 250 251 251 253 253 254 254 254 256

6.5.9 References

CONTENTS

8 Deformation Potentials 8.1 Intravalley Deformation Potential: Point 8.1.1 Group-IV Semiconductor Alloy 8.1.2 III–V Semiconductor Ternary Alloy (a) AlGaN (b) GaInN (c) AlInP (d) GaInP (e) AlGaAs (f) AlInAs (g) GaInAs (h) GaNAs (i) GaPAs 8.1.3 III–V Semiconductor Quaternary Alloy 8.1.4 II–VI Semiconductor Alloy 8.2 Intravalley Deformation Potential: High-symmetry Points 8.2.1 Group-IV Semiconductor Alloy 8.2.2 III–V Semiconductor Alloy 8.2.3 II–VI Semiconductor Alloy 8.3 Intervalley Deformation Potential 8.3.1 Group-IV Semiconductor Alloy 8.3.2 III–V Semiconductor Alloy 8.3.3 II–VI Semiconductor Alloy References 9 Heterojunction Band Offsets and Schottky Barrier Height 9.1 Heterojunction Band Offsets 9.1.1 General Considerations 9.1.2 Group-IV Semiconductor Heterostructure System (a) CSi/Si (b) SiGe/Si (c) CSiGe/Si (d) CSi/SiGe 9.1.3 III–V Semiconductor Heterostructure System: Lattice-matched Ternary-alloy System (a) GaInP/GaAs (b) GaInP/AlInP (c) GaInP/AlGaAs (d) AlGaAs/GaAs (e) AlInAs/InP (f) GaInAs/InP (g) GaInAs/AlInAs (h) InAsSb/GaSb 9.1.4 III–V Semiconductor Heterostructure System: Lattice-matched Quaternary Alloy (a) GaInPAs/InP

xi

259 259 259 261 261 262 262 263 263 264 265 265 266 266 266 267 267 269 270 270 270 271 272 272

275 275 275 275 275 276 276 277 277 277 277 278 278 279 279 280 280 280 280

xii

CONTENTS

(b) AlGaAsSb/GaSb (c) AlGaAsSb/InP (d) AlGaAsSb/InAs (e) GaInAsSb/GaSb (f) GaInAsSb/InP (g) GaInAsSb/InAs (h) AlGaAsSb/GaInAsSb (i) AlInAsSb/GaInAsSb (j) AlGaInP/AlInP (k) AlGaInP/GaInP (l) AlGaInAs/GaInAs 9.1.5 III–V Semiconductor Heterostructure System: Lattice-mismatched Alloy System (a) w-AlGaN/w-GaN (b) w-AlInN/w-InN (c) w-GaInN/w-GaN (d) GaInAs/GaAs (e) Dilute-nitride-based Heterostructure System 9.1.6 II–VI Semiconductor Heterostructure System (a) (II, II)–O-based Heterostructure System (b) (II, II)–S-based Heterostructure System (c) (II, II)–Se-based Heterostructure System (d) (II, II)–Te-based Heterostructure System (e) Zn–(VI, VI)-based Heterostructure System (f) (II, II)–VI-based and II–(VI, VI)-based Heterostructure Systems (g) (II, II)–(VI, VI)-based Heterostructure System (h) (II, II, II)–VI-based Heterostructure System 9.2 Schottky Barrier Height 9.2.1 General Considerations 9.2.2 Group-IV Semiconductor Alloy (a) SiGe Binary Alloy (b) CSiGe Ternary Alloy 9.2.3 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) (III, III)–Sb Alloy (e) Ga–(V, V) Alloy 9.2.4 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) Alloy (b) (III, III, III)–V Alloy 9.2.5 II–VI Semiconductor Alloy (a) (II, II)–Te Ternary Alloy (b) Zn–(VI, VI) Ternary Alloy References

281 281 281 281 281 281 282 282 282 282 283 283 283 284 284 284 286 287 287 287 287 288 289 289 289 289 289 289 290 290 291 291 291 292 292 294 295 296 296 297 299 299 300 300

CONTENTS

10 Optical Properties 10.1 Introductory Remarks 10.1.1 Optical Dispersion Relations 10.1.2 Static and High-frequency Dielectric Constants 10.2 Group-IV Semiconductor Alloy 10.2.1 Binary Alloy (a) CSi (b) CGe (c) SiGe (d) GeSn 10.2.2 Ternary Alloy 10.3 III–V Semiconductor Ternary Alloy 10.3.1 (III, III)–N Alloy (a) c-(III, III)–N Alloy (b) w-AlGaN (c) w-AlInN (d) w-GaInN 10.3.2 (III, III)–P Alloy (a) AlGaP (b) AlInP (c) GaInP 10.3.3 (III, III)–As Alloy (a) AlGaAs (b) AlInAs (c) GaInAs 10.3.4 (III, III)–Sb Alloy (a) AlGaSb (b) GaInSb 10.3.5 Dilute-nitride III–(V, V) Alloy (a) GaNP (b) GaNAs (c) GaNSb (d) InNP (e) InNAs 10.3.6 Al–(V, V) Alloy 10.3.7 Ga–(V, V) Alloy (a) GaPAs (b) GaPSb (c) GaAsSb 10.3.8 In–(V, V) Alloy (a) InPAs (b) InPSb (c) InAsSb 10.4 III–V Semiconductor Quaternary Alloy 10.4.1 Dilute-nitride Quaternary Alloy (a) GaInNP (b) GaInNAs

xiii

307 307 307 308 308 308 308 309 309 310 311 311 311 311 312 313 313 314 314 314 315 316 316 316 318 319 319 319 320 320 321 321 322 322 322 323 323 324 324 324 324 325 325 326 326 326 326

xiv

CONTENTS

10.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs (b) AlGaAsSb (c) GaInPAs (d) GaInAsSb 10.4.3 (III, III, III)–V Alloy (a) AlGaInP (b) AlGaInAs 10.4.4 III–(V, V, V) Alloy 10.5 II–VI Semiconductor Alloy 10.5.1 (II, II)–O Ternary Alloy (a) BeZnO (b) MgZnO (c) ZnCdO 10.5.2 (II, II)–S Ternary Alloy (a) MgZnS (b) ZnCdS 10.5.3 (II, II)–Se Ternary Alloy (a) BeZnSe (b) BeCdSe (c) MgZnSe (d) MgCdSe (e) ZnCdSe (f) CdHgSe 10.5.4 (II, II)–Te Ternary Alloy (a) BeZnTe (b) MgZnTe (c) MgCdTe (d) ZnCdTe (e) ZnHgTe (f) CdHgTe 10.5.5 Zn–(VI, VI) Ternary Alloy (a) ZnOS (b) ZnSSe (c) ZnSTe (d) ZnSeTe 10.5.6 Cd–(VI, VI) Ternary Alloy (a) CdSSe (b) CdSTe (c) CdSeTe 10.5.7 (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe (b) MgZnSeTe 10.5.8 (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe (b) BeZnCdSe (c) MgZnCdSe References

326 326 327 327 328 330 330 331 332 332 332 332 332 333 333 333 334 335 335 335 335 337 337 338 339 339 339 340 340 342 342 343 343 343 343 344 344 344 345 346 346 346 346 346 346 346 346 347

CONTENTS

xv

11 Elasto-optic, Electro-optic and Nonlinear Optical Properties 11.1 Elasto-optic Effect 11.1.1 Group-IV Semiconductor Alloy 11.1.2 III–V Semiconductor Alloy 11.1.3 II–VI Semiconductor Alloy 11.2 Linear Electro-optic Constant 11.2.1 Group-IV Semiconductor Alloy 11.2.2 III–V Semiconductor Alloy 11.2.3 II–VI Semiconductor Alloy 11.3 Quadratic Electro-optic Constant 11.3.1 Group-IV Semiconductor Alloy 11.3.2 III–V Semiconductor Alloy 11.3.3 II–VI Semiconductor Alloy 11.4 Franz–Keldysh Effect 11.4.1 Group-IV Semiconductor Alloy 11.4.2 III–V Semiconductor Alloy 11.4.3 II–VI Semiconductor Alloy 11.5 Nonlinear Optical Constant 11.5.1 Group-IV Semiconductor Alloy 11.5.2 III–V Semiconductor Alloy 11.5.3 II–VI Semiconductor Alloy References

357 357 357 357 357 358 358 358 358 360 360 360 360 360 360 360 360 361 361 361 362 362

12 Carrier Transport Properties 12.1 Introductory Remarks 12.2 Low-field Mobility 12.2.1 Group-IV Semiconductor Alloy (a) CSi Binary Alloy (b) SiGe Binary Alloy 12.2.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) (III, III)–Sb Alloy (e) Dilute-nitride III–(V, V) Alloy (f) Ga–(V, V) Alloy (g) In–(V, V) Alloy 12.2.3 III–V Semiconductor Quaternary Alloy (a) Dilute-nitride Alloy (b) (III, III)–(V, V) Alloy (c) (III, III, III)–V Alloy 12.2.4 II–VI Semiconductor Alloy (a) (II, II)–O Ternary Alloy (b) (II, II)–Se Ternary Alloy (c) (II, II)–Te Ternary Alloy (d) Zn–(V, V) Ternary Alloy

365 365 367 367 367 367 368 368 369 369 369 371 371 371 371 371 372 373 374 374 374 375 376

xvi

CONTENTS

12.3 High-field Transport 12.3.1 Group-IV Semiconductor Alloy 12.3.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) Dilute-nitride III–(V, V) Alloy 12.3.3 III–V Semiconductor Quaternary Alloy 12.3.4 II–VI Semiconductor Alloy 12.4 Minority-carrier Transport 12.4.1 Group-IV Semiconductor Alloy (a) SiGe Binary Alloy (b) CSiGe Ternary Alloy 12.4.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–As Alloy (c) Ga–(V, V) Alloy 12.4.3 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) Alloy (b) (III, III, III)–V Alloy 12.4.4 II–VI Semiconductor Alloy 12.5 Impact Ionization Coefficient 12.5.1 Group-IV Semiconductor Alloy 12.5.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N Alloy (b) (III, III)–P Alloy (c) (III, III)–As Alloy (d) (III, III)–Sb Alloy (e) Dilute-nitride III–(V, V) Alloy (f) Ga–(V, V) Alloy (g) In–(V, V) Alloy 12.5.3 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) Alloy (b) (III, III, III)–V Alloy 12.5.4 II–VI Semiconductor Alloy References Index

376 376 376 376 376 377 378 378 379 379 379 379 380 380 380 380 381 381 381 382 382 382 382 382 382 383 383 384 384 385 385 385 385 385 386 386 391

Preface Semiconductor alloys provide a natural means of tuning the magnitude of the band-gap energy and other material properties so as to optimize and widen the application of semiconductor devices. Current research and development in semiconductor alloys is focused on areas of improved materials growth, development of unique materials characterization and suitable process technologies, fabrication of novel devices using artificially controlled materials structures and better understanding of degradation mechanisms in electronic and optoelectronic devices for improved device reliability. Even though the basic semiconductor alloy concepts are understood at this time, the determination of some device parameters has been hampered by a lack of definite knowledge of many material parameters. The main purpose of this book is to provide a comprehensive treatment of the materials aspects of group-IV, III V and II VI semiconductor alloys used in various electronic and optoelectronic devices. The topics treated in this book include the structural, thermal, mechanical, lattice vibronic, electronic, optical and carrier transport properties of such semiconductor alloys. The book covers not only commonly known alloys (SiGe, AlGaAs, GaInPAs, ZnCdTe, etc.) but also new alloys, such as dilute-carbon alloys (CSiGe, CSiSn, etc.), III N alloys, dilute-nitride alloys (GaNAs, GaInNAs, etc.) and Mg- or Be-based II VI semiconductor alloys. The reader may also find the companion book Properties of Group-IV, III V and II VI Semiconductors published in this series useful since it emphasizes the endpoint semiconductor principles and properties. The extensive bibliography is included for those who wish to find additional information if required. It is hoped that the book will attract the attention of not only semiconductor device engineers, but also solid-state physicists and materials scientists, and particularly postgraduate students, R&D staff and teaching and research professionals. Sadao Adachi, Gunma University, Japan

Series Preface WILEY SERIES IN MATERIALS FOR ELECTRONIC AND OPTOELECTRONIC APPLICATIONS This book series is devoted to the rapidly developing class of materials used for electronic and optoelectronic applications. It is designed to provide much-needed information on the fundamental scientific principles of these materials, together with how these are employed in technological applications. The books are aimed at (postgraduate) students, researchers and technologists, engaged in research, development and the study of materials in electronics and photonics, and industrial scientists developing new materials, devices and circuits for the electronic, optoelectronic and communications industries. The development of new electronic and optoelectronic materials depends not only on materials engineering at a practical level, but also on a clear understanding of the properties of materials, and the fundamental science behind these properties. It is the properties of a material that eventually determine its usefulness in an application. The series therefore also includes such titles as electrical conduction in solids, optical properties, thermal properties, and so on, all with applications and examples of materials in electronics and optoelectronics. The characterization of materials is also covered within the series in as much as it is impossible to develop new materials without the proper characterization of their structure and properties. Structure-property relationships have always been fundamentally and intrinsically important to materials science and engineering. Materials science is well known for being one of the most interdisciplinary sciences. It is the interdisciplinary aspect of materials science that has led to many exciting discoveries, new materials and new applications. It is not unusual to find scientists with a chemical engineering background working on materials projects with applications in electronics. In selecting titles for the series, we have tried to maintain the interdisciplinary aspect of the field, and hence its excitement to researchers in this field. Peter Capper Safa Kasap Arthur Willoughby

Abbreviations and Acronyms BAC bct BZ

band anticrossing body-centered tetragonal Brillouin zone

cCB CL Cl-VPE CP CR C–V CVD

cubicconduction band cathodoluminescence chloride-transport vapor-phase epitaxy critical point cyclotron resonance capacitance–voltage chemical vapor deposition

DLTS DOS DP

deep-level transient spectroscopy density of states deformation potential

ER EXAFS

electroreflectance extended X-ray absorption fine-structure spectroscopy

fcc FET FTIR

face-centered cubic field effect transistor Fourier transform infrared

HBT HH HREELS HRXRD HT-VPE

heterojunction bipolar transistor heavy-hole high-resolution electron-energy-loss spectroscopy high-resolution X-ray diffraction hydride-transport vapor-phase epitaxy

IR I–V

infrared current–voltage

LA LH LO LPE

longitudinal acoustic light-hole longitudinal optical liquid-phase epitaxy

MBE MDF MOCVD

molecular beam epitaxy model dielectric function metalorganic chemical vapor deposition

xxii

ABBREVIATIONS AND ACRONYMS

MOMBE MQW MREI

metalorganic molecular beam epitaxy multiple quantum well modified random-element-isodisplacement

PDP PIXE PL PLD PLE PR PzR

phonon deformation potential particle-induced X-ray emission photoluminescence pulsed-laser deposition photoluminescence excitation photoreflectance piezoreflectance

QW

quantum well

RBS rf RHEED

Rutherford backscattering spectrometry radio-frequency reflection high-energy electron diffraction

SE SL SO

spectroscopic ellipsometry superlattice spin–orbit

TA TEM THM TO TP TR

transverse acoustic transmission electron microscopy traveling heater method transverse optical triple-period thermoreflectance

UHV UV

ultrahigh vacuum ultraviolet

VB VCA VPE

valence band virtual crystal approximation vapor-phase epitaxy

wWDXS

wurtzite wavelength-dispersive X-ray spectroscopy

XPS XRD

X-ray photoelectron spectroscopy X-ray diffraction

1D 2D 3D

one-dimensional two-dimensional three-dimensional

Introductory Remarks A.1 AN ALLOY AND A COMPOUND An alloy is a combination, either in solution or compound, of two or more elements. An alloy with two components is called a binary alloy; one with three is a ternary alloy; one with four is a quaternary alloy; one with five is a pentanary alloy. The resulting alloy substance generally has properties significantly different from those of its components. The proportions of the ingredients are available. A chemical compound is a substance consisting of two or more chemical elements that are chemically combined in fixed proportions. The ratio of each element is usually expressed by chemical formula. For example, water is a compound consisting of two hydrogen atoms bonded to an oxygen atom (H2O). The atoms within a compound can be held together by a variety of interactions, ranging from covalent bonds to electrostatic forces in ionic bonds. A continuum of bond polarities exists between the purely covalent and ionic bonds. For example, H2O is held together by polar covalent bonds. NaCl is an example of an ionic compound. Simply, an alloy is formed from a physical mixture of two or more substances, while a compound is formed from a chemical reaction. An alloy crystal is sometimes called a mixed crystal or a solid solution. For example, GaAs is a compound consisting of Ga atoms bonded to As atoms. It is not an alloy. AlxGa1xAs is an alloy compound consisting of AlAs and GaAs with a mole ratio of x:(1 x). The bonds in GaAs and AlAs are not adequately described by any of these extreme types, but have characteristics intermediate to those usually associated with the covalent and ionic terms. The bonds in diamond, CC, can be described by the covalent bond term only. It is an elemental semiconductor, not a compound semiconductor. Similarly, Si and Ge are elemental semiconductors. Like AlxGa1xAs, SixGe1x (0 x 1.0) is an alloy semiconductor. The bonds SiGe, SiSi and GeGe in SixGe1x are, therefore, described by the covalent term only. It should be noted, however, that silicon carbide (SiC) is a compound, not an alloy. This is because that the chemical bonds in SiC cannot be described only by the covalent term, but have characteristics intermediate to those associated with the covalent and ionic terms, like GaAs and AlAs. There is an ordered alloy phase in SixGe1x binary alloy [1]. This phase exhibits long-range order rather than random arrangement of atoms as expected previously. The ordered phase, as expected, occurs mostly in bulk SixGe1x layers at x 0.5 and can be explained by the rhombohedral structure. Note that SiC is thought to be an ordered alloy. It crystallizes in a large number of polytypes. The various types of SiC differ one from another only by the order in which successive planes of Si (or C) atoms are stacked along the c axis; one polytype is the cubic, zinc-blende structure (3C) while the reminder, including two of the more frequently occurring forms, 6H (hexagonal) and 15R (rhombohedral), possess uniaxial symmetry [2]. There is no diamond structure in the SiC polytypes. An ordered alloy phase has been found not only in SixGe1x, but also in many III–V and II–VI semiconductor alloys [3]. Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

2

PROPERTIES OF SEMICONDUCTOR ALLOYS

A.2 GRIMM–SOMMERFELD RULE The periodic law is most commonly expressed in chemistry in the form of a periodic table or chart. An important part of this table is shown in Table A.1. The so-called short-form periodic table, based on the Mendeleyev table, with subsequent emendations and additions, is still in widespread use. The elements in this table are arranged in seven horizontal rows, called the periods, in order of increasing atomic weights, and in 18 vertical columns, called the groups. The first period, containing two elements, H and He, and the next two periods, each containing eight elements, are called the short periods. The remaining periods, called the long periods, contain 18 elements, as in periods 4 and 5, or 32 elements, as in period 6. The long period 7 includes the actinide series, which has been filled in by the synthesis of radioactive nuclei through element 103, lawrencium (Lr). Heavier transuranium elements, atomic numbers 104 to 112, have also been synthesized. Table A.1 Periodic table

The elemental semiconductors in column IVa of the periodic table are diamond, Si and Ge, and they are of some importance in various device applications. Note that gray tin (a-Sn) is a semiconductor (semimetal) and Pb is a metal. SiC is the only compound semiconductor formed by column IVa elements. The III–V and II–VI semiconductors possess a crystal structure similar to either one of the cubic mineral, sphalerite or to hexagonal wurtzite. There are 15 III–V, 18 II–VI and four I–VII compound semiconductors. The four I–VII compound semiconductors are: CuCl, CuBr, CuI and AgI. A substantial development in the search for semiconducting materials with new combinations of physical and chemical properties was reached when Goryunova using the ideas of Huggins [4] and Grimm and Sommerfeld [5], developed a method of prediction of the composition of chemical compounds with the tetrahedral and octahedral (NaCl-type) coordination of atoms in their crystal lattice [6]. His method is based on consideration of the number of valence electrons in the elements, which is assumed to be equal to the number of the group in

INTRODUCTORY REMARKS

3

the periodic table to which they belong (so-called full or normal valency) and can be expressed in the form of the equation system [7] A X i¼1 n X i¼1 A X

Bi x i ¼ 4 Bi x i ¼

A X

ð8Bi Þxi

ðA:1Þ

i¼nþ1

xi ¼ 1

i¼1

for calculating the content of the representatives of different groups of the periodic table in a compound containing A components, n of which are considered as cations, where Bi is the number of the group in the periodic table to which the ith component of the compounds belongs, and xi is its concentration in the compound. The first expression in Equation (A.1) represents the condition that the average number of valence electrons per atom is equal to four (tetrahedral rule). The second equation states that in the compound, the number of valence electrons, which cations give to anions is equal to the number of electrons the anion needs to form the octet (i.e. the normal valency condition). The quotation marks here are used to remind us that in the solids with dominating covalent bonds, which factually form the class of semiconductor, the ion concept is quite conditional. Based on these criteria, it is possible to obtain all probable types of tetrahedral substances, taking into consideration only the location of their components in one or another group of the periodic table. Table A.2 briefly summarizes these results. Table A.2 Summary of valence binary compounds and ternary analogs of binary valence compounds which satisfy tetrarahedral rule (Z¼4). ch¼chalcopyrite; zb¼zinc-blende; t¼tetragonal; or¼orthorhombic; w¼wurtzite; h¼hexagonal (P63mc (C6v)); rh¼rhombohedral Cation

Compound

Typical compound (Crystal structure)

I

I–III–VI2 I–IV2–V3 I2–IV–VI3 I3–V–VI4 I–VII

CuGaSe2 (ch) CuGe2P3 (zb) Cu2GeSe3 (t) Cu3PS4 (or) g-CuCl (w)

II

II4–III–VII3 II–IV–V2 II3–IV–VII2 II2–V–VII II–VI

III

IV

ZnSiP2 (ch) CdTe (zb)

III2–IV–VI III3–IV2–VII III–V

GaAs (zb)

IV–IV

SiC (zb, w, h, rh)

Al2CO (w)

4

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table A.3 All the possible types of valence binary compound Cation

Cation to anion content ratio x/y, (Z), Typical compound II

I

6:1 (1.14)

III

IV

V

5:1 (1.33)

4:1 (1.60)

5:2 (2.29)

2:1 (2.67) Mg2Si 4:3 (3.43)

II

—

III

—

—

IV

—

—

V

—

—

VI

—

—

1:1 (4.00) SiC — —

3:1 (2.00) K3Sb 3:2 (3.20) Cd3As2 1:1 (4.00) GaAs 3:4 (4.57) — —

VI 2:1 (2.67) Ag2S 1:1 (4.00) CdTe 2:3 (4.80) Ga2Se3 1:2 (5.33) SnS2 2:5 (5.71) —

VII 1:1 (4.00) g-CuCl 1:2 (5.33) HgI2 1:3 (6.00) 1:4 (6.40) 1:5 (6.67) 1:6 (6.86)

In analyzing the normal valency compounds, not only tetrahedral phases but all compounds of this category can be grouped, first of all, in accordance with the average valence electron content per atom of a compound, Z. We list in Table A.3 all possible types of the binary valence compounds [7]. If A and B are the cation valencies in a binary compound, the atomic ratio of components in a valence compound AxBy is given by x 8B ¼ y A

ðA:2Þ

and the valence electron concentration per atom in the corresponding binary compound is Z¼

8A 8A ¼ 8ðBAÞ 8þðABÞ

ðA:3Þ

as following from Equation (A.1). In Table A.3, there are 22 types of binary valence compounds. Goryunova [6] concluded from the available experimental data that the phases possessing semiconducting properties are those with Z between two and six; the phases smaller than two are either metal alloys or the compounds with typical metallic crystal structure and properties. Goryunova also showed that there are 148 types of ternary compounds which are the electron analogs of the binary valence compounds [7]. Among them, there are 10 types of ternary compounds which satisfy the tetrarahedral rule Z ¼ 4, as listed in Table A.2.

A.3 AN INTERPOLATION SCHEME The electronic energy-band parameters of semiconductor alloys and their dependence on alloy compositionareveryimportant,andsotheyhavereceivedmuchattentioninthepast.Investigation

INTRODUCTORY REMARKS

5

of many device parameters have, however, been hampered by a lack of definite knowledge of various material parameters. This necessitates the use of some sort of interpolation scheme. If the linear interpolation scheme is used, the ternary material parameter T for an alloy of the form AxB1xC can be derived from binary parameters (B) by TðxÞ ¼ xBAC þð1xÞBBC aþbx

ðA:4Þ

where a BBC and b BAC BBC. Some material parameters, however, deviate significantly from the linear relationship shown in Equation (A.4), and exhibit an approximately quadratic dependence on x. The ternary material parameter in such a case can be very efficiently approximated by the relationship TðxÞ ¼ xBAC þð1xÞBBC þxð1xÞCAB aþbxþcx2

ðA:5Þ

where a BBC, b BAC BBC þ CAB and c CAB. The parameter c is called a bowing parameter. The quaternary material AxB1xCyD1y is thought to be constructed from four binaries: AC, AD, BC and BD. If the linear interpolation scheme is used, the quaternary material parameter Q can be derived from the binary parameters by Qðx;yÞ ¼ xyBAC þxð1yÞBAD þð1xÞyBBC þð1xÞð1yÞBBD

ðA:6Þ

If one of the four binary parameters (e.g. BAD) is lacking, Q can be estimated from Qðx;yÞ ¼ xBAC þðyxÞBBC þð1yÞBBD

ðA:7Þ

The quaternary material AxByC1xyD is thought to be constructed from three binaries: AD, BD and CD. The corresponding linear interpolation is given by Qðx;yÞ ¼ xBAD þyBBD þð1xyÞBCD

ðA:8Þ

If relationships for the ternary parameters are available, the quaternary material parameter Q can be expressed either as (AxB1xCyD1y) Qðx;yÞ ¼

xð1xÞ½yTABC ðxÞþð1yÞTABD ðxÞþyð1yÞ½xTACD ðyÞþð1xÞTBCD ðyÞ xð1xÞþyð1yÞ

ðA:9Þ

or (AxByC1xyD) Qðx;yÞ ¼

xyTABD ðuÞþyð1xyÞTBCD ðvÞþxð1xyÞTACD ðwÞ xyþyð1xyÞþxð1xyÞ

ðA:10Þ

with u ¼ ð1xyÞ=2 v ¼ ð2x2yÞ=2 w ¼ ð22xyÞ=2

ðA:11Þ

6

PROPERTIES OF SEMICONDUCTOR ALLOYS

If a quaternary bowing term DABCD ¼ d is considered in Equation (A.9) or Equation (A.10), we can obtain Qðx;yÞ ¼ fxð1xÞ½yTABC ðxÞþð1yÞTABD ðxÞþyð1yÞDABCD þyð1yÞ ½xTACD ðyÞþð1xÞTBCD ðyÞþxð1xÞDABCD g½xð1xÞþyð1yÞ1

; ðA:12Þ

for the AxB1xCyD1y quaternary or Qðx;yÞ ¼

xyTABD ðuÞþyð1xyÞTBCD ðvÞþxð1xyÞTACD ðwÞþxyð1xyÞDABCD ðA:13Þ xyþyð1xyÞþxð1xyÞ

for the AxByC1xyD quaternary. The weighted form of Equation (A.12) can be written as Qðx;yÞ ¼ yð1xÞBBC þxyBAC þð1yÞxBAD þð1xÞð1yÞBCD þxð1xÞð1yÞCABðDÞ þxð1xÞyCABðCÞ þð1xÞyð1yÞCðBÞCD þxyð1yÞCðAÞCD þxð1xÞyð1yÞDABCD

ðA:14Þ

where CAB(D) is the ternary bowing parameter for an alloy AxB1xD and so on. Expression (A.14) can be conveniently compacted into an inner product whose 3 3 matrix includes only the alloy parameters and closely resembles the map of the quaternary alloy in its compositional space [8] 2 32 3 BBC CABðCÞ BAC 1x Qðx;yÞ ¼ ½ y yð1yÞ 1y 4 CðBÞCD DABCD CðAÞCD 54 xð1xÞ 5 ðA:15Þ BBD CABðDÞ BAD x If the bowing parameters C and D in Equation (A.15) are zero, Vegard law is recovered in its bilinear formulation. Equation (A.15) is valid for quaternaries of types AxB1xCyD1y and AxByC1xyD (ABxCyD1xy). For the latter, one binary can be assigned twice in the same raw or column of the alloy matrix with a zero bowing factor (i.e. BAC ¼ BAD and C(A)CD ¼ 0). The composition for such an alloy is given by (BAD)x[(BBD)y(BCD)1y]1x (e.g., Alx(GayIn1y)1xP). The essentially same expressions can be obtained for group-IV semiconductor alloys. The binary material parameter B in the form of AxB1x can be written using the elemental material parameters (A) as BðxÞ ¼ xAA þð1xÞAB aþbx

ðA:16Þ

The bowing effect modifies Equation (A.16) in the form BðxÞ ¼ xAA þð1xÞAB þxð1xÞCAB aþbxþcx2

ðA:17Þ

Similarly, the ternary material parameter T in AxByC1xy can be expressed as Tðx;yÞ ¼ xAA þyAB þð1xyÞAC

ðA:18Þ

INTRODUCTORY REMARKS

7

and Tðx;yÞ ¼

xyBAB ðuÞþyð1xyÞBBC ðvÞþxð1xyÞBAC ðwÞ xyþyð1xyÞþxð1xyÞ

ðA:19Þ

or Tðx;yÞ ¼

xyBAB ðuÞþyð1xyÞBBC ðvÞþxð1xyÞBAC ðwÞþxyð1xyÞCABC xyþyð1xyÞþxð1xyÞ

ðA:20Þ

with u, v and w given in Equation (A.11). In Equation (A.20), CABC is a ternary bowing parameter.

REFERENCES [1] W. J€ager, in Properties of Strained and Relaxed Silicon Germanium, EMIS Datareviews Series No. 12 (edited by E. Kasper), INSPEC, London, 1995, p. 53. [2] S. Adachi, Properties of Group-IV, III-V and II-VI Semiconductors. John Wiley & Sons, Ltd, Chichester, 2005. [3] A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys. Kluwer Academic, New York, 2002. [4] M. L. Huggins, Phys. Rev. 27, 286 (1926). [5] H. Grimm and A. Sommerfeld, Z. Phys. 36, 36 (1926). [6] N. A. Goryunova, The Chemistry of Diamond-Like Semiconductors. MIT Press, Cambridge, 1965. [7] L. I. Berger, Semiconductor Materials. CRC, Boca Raton, 1997. [8] G. P. Donati, R. Kaspi, and K. J. Malloy, J. Appl. Phys. 94, 5814 (2003).

1 Structural Properties 1.1 IONICITY Details of ionicity fi are given in Adachi [1]. Any given definition of ionicity is likely to be imperfect. We present in Table 1.1 fi values for a number of group-IV, III–V and II–VI semiconductors, including Be-based semiconductors and CdO. We have Phillips ionicity of fi ¼ 0 for all group-IV elemental semiconductors (diamond, Si, Ge and a-Sn) and fi > 0.9 for some alkali halides (NaCl, KCl, etc.). Figure 1.1(a) plots fi versus x for CxSi1x. Note that fi ¼ 0.177 for silicon carbide (SiC). This means that the bond character of SiC resembles that of III–V or II–VI semiconductors rather than of Si or diamond, so that its crystal structure must be zinc-blende, hexagonal or rhombohedral. Similarly, an ordered alloy of SixGe1x may have a nonzero fi value near the ordered-phase composition x 0.5. In fully disordered alloys (CxSi1x, SixGe1x, etc.), we should have fi ¼ 0 over the whole alloy range 0 x 1.0. The plots of fi versus x or y for AlxGa1xAs, GaxIn1xPyAs1y/InP and MgxZn1xSySe1y/GaAs are shown in Figure 1.1(b). These values are obtained from the linear interpolation of Equations (A.4) and (A.6) between the endpoint data in Table 1.1. The resulting fi versus x (y) plots can be expressed in the usual power form as fi ðxÞ ¼ 0:310 0:036x

ð1:1aÞ

fi ðyÞ ¼ 0:335 þ 0:065y þ 0:021y2

ð1:1bÞ

fi ðxÞ ¼ 0:630 þ 0:154x þ 0:003x2

ð1:1cÞ

for AlxGa1xAs, for GaxIn1xPyAs1y/InP and for MgxZn1xSySe1y/GaAs. The values of fi for fully disordered alloys should be safely estimated from the linear interpolation scheme.

1.2 ELEMENTAL ISOTOPIC ABUNDANCE AND MOLECULAR WEIGHT In Tables 1.2 and 1.3 of Adachi [1], the elements which form at least one tetrahedrally coordinated ANB8N semiconductor, together with their natural isotopic abundance in percent and atomic weight are listed. Let us add an element of beryllium: natural abundance of 9 Be ¼ 100%; atomic weight ¼ 9.012182(3).

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

10

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.1 Phillips’s ionicity fi for a number of group-IV, III–V and II–VI semiconductors IV Diamond Si Ge Sn SiC

fi

III–V

fi

II–VI

fi

0 0 0 0 0.177

BN BP BAs AlN AlP AlAs AlSb GaN GaP GaAs GaSb InN InP InAs InSb

0.221 0.032 0.044 0.449 0.307 0.274 0.250 0.500 0.327 0.310 0.261 0.578 0.421 0.357 0.321

BeO BeS BeSe BeTe MgO MgS MgSe MgTe ZnO ZnS ZnSe ZnTe CdO CdS CdSe CdTe HgS HgSe HgTe

0.602 0.286 0.261 0.169 0.841 0.786 0.790 0.554 0.616 0.623 0.630 0.609 0.785 0.685 0.699 0.717 0.790 0.680 0.650

The molecular weight M for an ANB8N compound semiconductor (N„ 4) can be simply given by the sum of the atomic weights of atoms A and B. For an elemental semiconductor (N ¼ 4), it is given by the atomic weight of the element atom A ¼ B. The molecular weight M of any alloy semiconductors can be obtained from the linear interpolation scheme. 0.25 CxSi1-x

fi

0.20

(a)

SiC

0.15 Ordered alloy

0.10 0.05 0

0

0.2

0.4

1.0

x

0.6

0.8

1.0

Mgx Zn1-x SySe1-y /GaAs (x)

0.8 fi

Disordered alloy

0.6 Gax In1-x Py As1-y /InP (y)

0.4 0.2 0

AlxGa1-x As

(b) 0

0.2

0.4

0.6 x or y

0.8

1.0

Figure 1.1 Phillips ionicity fi versus x or y for (a) CxSi1x and (b) AlxGa1xAs, GaxIn1xPyAs1y/InP and MgxZn1xSySe1y/GaAs. The open and solid circles in (a) show the endpoint and SiC (x ¼ 0.5) values, respectively. The solid lines in (b) are calculated from Equation (1.1)

STRUCTURAL PROPERTIES

11

1.3 CRYSTAL STRUCTURE 1.3.1 Random Alloy Table 1.2 summarizes the crystal classes for easily obtained or normally grown: (a) group-IV elemental semiconductors, (b) III–V and (c) II–VI binary semiconductors. In Table 1.2(a), the crystal classes for an easily grown compound semiconductor SiC are also included. Table 1.2 Summary of crystal structure for: (a) group-IV, (b) III–V and (c) II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite (C6v); h ¼ hexagonal (C6v or D6h); rh ¼ rhombohedral; t ¼ tetragonal; rs ¼ rocksalt; or ¼ orthorhombic. Note that b-Sn (t) is a metal (a) IV

C

Si

C Si Ge Sn

d zb, w, h, rh

zb, w, h, rh d

Ge

d

Sn

d, t

(b) III/V

N

P

As

Sb

B Al Ga In

zb, h w w w

zb zb zb zb

zb zb zb zb

zb zb zb

(c) II/VI

O

S

Se

Te

Be Mg Zn Cd Hg

w rs w rs rh, or

zb rs zb, w w zb, rh

zb zb zb w zb

zb w zb zb zb

1.3.2 Spontaneous Ordering (a) Group-IV semiconductor alloy The phenomenon of spontaneous ordering in semiconductor alloys is observed to occur spontaneously during epitaxial growth of certain semiconductor alloys and results in a modification of their structural, electronic and optical properties [2]. Substantial effort has been focused on learning how to control this phenomenon so that it may be used for tailoring desirable material properties. We summarize in Table 1.3 the spontaneous ordering phases observed in some group-IV, III–V and II–VI semiconductor alloys.

12

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.3 Types of spontaneous ordering phases observed in some group-IV, III–V and II–VI semiconductor alloys System

Ordering type

Material

Epitaxial growth

IV

RS1 (CuPt) RS2 (CuPt) RS3 (CuPt)

SiGe SiGe SiGe

MBEa MBEa MBEa

III–V

CuPt-B

AlInP GaInP AlInAs GaInAs GaInSb GaPAs GaPSb GaAsSb InPAs InPSb InAsSb GaInPAs AlGaInP AlInP AlInAs AlGaAs GaInAs GaAsSb AlInAs GaInAs

MBE,b MOCVDc Cl-VPE,d HT-VPE,e MBE,f MOCVDg MEB,h MOCVDi Cl-VPE,j MOCVDk MOCVDl MOCVDm MOCVDn MBEo MOCVDp MOCVDq MOCVD,r MBEs Cl-VPE,j MOCVDt MOCVDc MBEb MBEu MOCVDv MBEw MBE,x MOCVDy MBEz MBEaa

ZnCdTe CdHgTe ZnSeTe ZnCdTe ZnSeTe ZnCdTe

MOCVDab LPEac MOCVDad MBEae MBEaf MBEag

CuPt-A CuAu-I TP-A

II–VI

CuPt-B CuAu-I Cu3Au

See, W. J€ager, in Properties of Strained and Relaxed Silicon Germanium, EMIS Datareviews Series No. 12 (edited by E. Kasper), INSPEC, London, 1995, p. 53 b A. Gomyo et al., Jpn. J. Appl. Phys. 34, L469 (1995) c T. Suzuki et al., Jpn. J. Appl. Phys. 27, 2098 (1988) d O. Ueta et al., J. Appl. Phys. 68, 4268 (1990) e K. Nishi and T. Suzuki (unpublished) f A. Gomyo et al., Mater. Res. Symp. Proc. 417, 91 (1996) g A. Gomyo et al., Phys. Rev. Lett. 60, 2645 (1988) h T. Suzuki et al., Appl. Phys. Lett. 73, 2588 (1998) i A. G. Norman et al., Inst. Phys. Conf. Ser. 87, 77 (1987) j M. A. Shahid et al., Phys. Rev. Lett. 58, 2567 (1987) k T.-Y. Seong et al., J. Appl. Phys. 75, 7852 (1994) l J. Shin et al., J. Electron. Mater. 24, 1563 (1995) m G. S. Chen et al., Appl. Phys. Lett. 57, 2475 (1990) n G. B. Stringfellow, J. Cryst. Growth 98, 108 (1989) a

STRUCTURAL PROPERTIES

13

Figure 1.2 Si–Ge ordered structures of types (a) RS1, (b) RS2 and (c) RS3. In (c), the four projected compositions a, b, g and d correspond to specific Si- and Ge-rich sites

Normally, SixGe1x crystallizes in the diamond structure which contains of two fcc sublattices shifted by one quarter of the body diagonal. Observations of long-range ordering of group-IV semiconductor alloy have been made on SixGe1x layers grown on Si(100) by MEB [3] and subsequently at interfaces of SLs [2]. Different order structures were suggested in bulk SixGe1x on the basis of experimental results and are depicted in Figure 1.2. They are RS1, RS2 and RS3 with the rhombohedral structures (CuPt ordering, R3m). The stoichiometry for RS1 and RS2 is Si0.5Ge0.5, while RS3 allows compositional differences on specific lattice sites. As seen in Figure 1.2, RS1 (RS2) has the widely (closely) spaced {111} planes occupied by the same atom type, while RS3 allows compositional differences between projected sites or columns with compositions a, b, g and d corresponding to specific Si- and Ge-rich sites.

3 Y.-E. Ihm et al., Appl. Phys. Lett. 51, 2013 (1987) D. H. Jaw et al., Appl. Phys. Lett. 59, 114 (1991) q See, H. R. Jen et al., Appl. Phys. Lett. 54, 1890 (1989) r H. R. Jen et al., Appl. Phys. Lett. 54, 1154 (1989) s T.-Y. Seong et al., Appl. Phys. Lett. 64, 3593 (1994) t W. E. Plano et al., Appl. Phys. Lett. 53, 2537 (1988) u T. Suzuki et al., Appl. Phys. Lett. 73, 2588 (1998) v T. S. Kuan et al., Phys. Rev. Lett. 54, 201 (1985) w O. Ueda, et. al., J. Cryst. Growth 115, 375 (1991) x O. Ueta et al., Proc. 7th Int. Conf. InP and Related Materials Sapporo, Japan, p. 253 (1995) y H. R. Jen et al., Appl. Phys. Lett. 48, 1603 (1986) z A. Gomyo et al., Phys. Rev. Lett. 72, 673 (1994) aa D. Shindo et al., J. Electron Microscopy 45, 99 (1996) ab N. Amir et al., J. Phys. D: Appl. Phys. 33, L9 (2000) ac K. T. Chang and E. Goo, J. Vac. Sci. Technol. B 10, 1549 (1992) ad K. Wolf et al., Solid State Commun. 94, 103 (1995) ae H. S. Lee et al., Appl. Phys. Lett. 83, 896 (2003) af H. Luo et al., J. Vac. Sci. Technol. B 12, 1140 (1994) ag H. S. Lee et al., Solid State Commun. 137, 70 (2006) o p

14

PROPERTIES OF SEMICONDUCTOR ALLOYS

The long-range order parameter in RS1 and RS2 can be defined by rSi x S¼ 1x

ð1:2Þ

where rSi is the fraction of Si sites occupied correctly and x is the fraction of Si atoms in SixGe1x. S ¼ 1 means perfect and complete order, while S ¼ 0 means random alloy. The degree of long-range order can be quantitatively deduced from the electron diffraction intensity of superstructure reflections. However, because of the presence of crystalline defects, of superposition of various domains and of the multiple scattering, the actual intensity substantially deviates from the kinematic value so that quantitative determination from selected-area electron diffraction intensity is usually obscured [2]. Observations of the long-range ordering have been made on bulk SiGe or SL samples prepared by MBE at medium temperature and for various compositions. However, no observations of ordered phases are reported for bulk SiGe grown from the melt [4]. (b) III–V semiconductor alloy In 1985, Kuan et al. [5] first observed an ordered phase (CuAu-I type) in III–V semiconductor alloy which was an AlGaAs epilayer grown on GaAs(100) at 600–800 C by MOCVD. Since the finding of CuPt-type ordering in SiGe alloy [3], this type of ordering (CuPt-B) has also been reported for many III–V alloys, such as AlInP, GaInP, AlInAs and GaInAs ([6], see also Table 1.3). New types of ordering, CuPt-A and TP-A, are also found in AlInP [7] and AlInAs alloys [8]. Other types of ordering, CuAu-I, famatinite and chalcopyrite, are reported in the early history of the spontaneous ordering in III–Valloys; however, mechanism of these phases seems to be quite different from those of CuPt-B, CuPt-A and TP-A [6]. The unit cells of (a) CuPt-B, (b) CuAu-I and (c) chalcopyrite structures are shown in Figure 1.3. The metallurgical CuPt alloy has a random fcc structure at high temperatures, but quenching at low temperatures produces a rhombohedral phase with 1/2{111} chemical ordering. The CuPt-B structure is among the most widely discussed and accessed forms of spontaneous ordering in III–V ternaries, and occurs in both common anion and common cation alloys (Table 1.3). It is a monolayer SL of IIIA (VA)-rich planes and IIIB (VB)-rich planes ordered in the ½ 111 or ½1 11 directions, as depicted in Figure 1.4. The CuPt-A and

Figure 1.3 Unit cells of (a) CuPt-B (GaInAs), (b) CuAu-I (AlGaAs) and (c) chalcopyrite structures (CuGaSe2)

STRUCTURAL PROPERTIES

15

Figure 1.4 [110] projection of CuPt-B ordering (GaInP)

1 1 and ½111 directions, in which CuPt-B ordering is never TP-A phases occur in the ½1 observed. The metallic CuAu alloy shows two prominent ordered phases: (i) CuAu-I trigonal phase with alternating (002) planes of pure Cu and Au compositions and (ii) orthorhombic CuAu-II phase. The CuAu-I ordering occurs spontaneously within fcc sublattices of some III–V pseudobinary alloys, such as AlGaAs, GaInAs and GaAsSb (Table 1.3). An earlier thermodynamic calculation based on a first-principles theory predicted that an ordered phase with a large lattice-constant mismatch is more stable than the corresponding random phase [9]. Some experimental data, on the other hand, showed that the kinetics of crystal growth plays an important role in the formation of an ordered structure as discussed in Mascarenhas [2]. (c) II–VI semiconductor alloy Only a few studies have been carried out on spontaneous ordering of II–VI semiconductor alloys. These studies reported ordering of CuPt and CuAu-I types (Table 1.3). Recently, a new ordering phase, Cu3Au, has been observed in Zn0.9Cd0.1Te epilayers grown on GaAs(100) substrates [10]. We can see a tendency in Table 1.3 to observe the CuPt (CuAu-I) phase if samples were grown by MOCVD (MBE).

1.4 LATTICE CONSTANT AND RELATED PARAMETERS 1.4.1 CuAu Alloy: Ordered and Disordered States Cu–Au alloy is among the best studied of all metallic alloys. The most interesting feature of this alloy is that CuAu (x ¼ 0.5), CuAu3 (x ¼ 0.25) and Cu3Au (x ¼ 0.75) can be obtained in either ordered or disordered form. The ordered CuAu alloy crystallizes in the LI0 tetragonal structure

16

PROPERTIES OF SEMICONDUCTOR ALLOYS 5.0 Cux Au1-x

a (Å)

4.5 4.0 3.5

CuAu3 (LI2) Cu3Au (LI2)

3.0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.5 Lattice constant a versus x for CuxAu1x. The solid and open circles represent the ordered (x ¼ 0.25, 0.75) and disordered alloy values, respectively. The solid line shows the linear interpolation result between the endpoint elemental data

(space group ¼ P4/mmm), while the ordered CuAu3 and Cu3Au alloys crystallize in the LI2 cubic structure ðPm 3mÞ. In Figure 1.5 the lattice constant a has been plotted as a function of x for CuxAu1x. The solid and open circles represent the ordered and disordered alloy data, respectively. The solid line shows the linear interpolation result between the Au (x ¼ 0) and Cu (x ¼ 1.0) values. It can be seen from Figure 1.5 that the Cu–Au ordering has no strong effect on the lattice parameter. Similarly, no clear spontaneous ordering effect has been observed on the lattice parameters of semiconductor alloys.

1.4.2 Non-alloyed Semiconductor The lattice parameters for a number of the most easily grown group-IV, III–V and II–VI semiconductors are listed in Table 1.4. Tables 1.5, 1.6 and 1.7 also list the molecular weight (M), lattice constants (a and b) and crystal density (g) for a number of group-VI, III–Vand II–VI semiconductors crystallizing in the diamond, zinc-blende and wurtzite structures, respectively. These values can be used to obtain alloy values using the interpolation scheme.

Table 1.4 Most easily grown crystal structure and lattice constants at 300 K for a number of easily or normally grown group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; h ¼ hexagonal; w ¼ wurtzite; rs ¼ rocksalt; or ¼ orthorhombic; rh ¼ rhombohedral

System

Material

Crystal structure

a (A)

c (A)

IV

Diamond Si Ge Sn 3C-SiC 6H-SiC

d d d d zb h

3.5670 5.4310 5.6579 6.4892 4.3596 3.0806

15.1173

System

Material

Crystal structure

a (A)

c (A)

STRUCTURAL PROPERTIES

17

Table 1.4 (Continued )

System

Material

Crystal structure

a (A)

III–V

BN BN BP BAs AlN AlP AlAs AlSb GaN GaP GaAs GaSb InN InP InAs InSb

zb h zb zb h (w) zb zb zb h (w) zb zb zb h (w) zb zb zb

3.6155 2.5040 4.5383 4.777 3.112 5.4635 5.66139 6.1355 3.1896 5.4508 5.65330 6.09593 3.548 5.8690 6.0583 6.47937

BeO BeS BeSe BeTe MgO MgS MgSe MgTe ZnO ZnS ZnS ZnSe ZnTe CdO CdS CdSe CdTe HgO

h (w) zb zb zb rs rs zb h (w) h (w) h (w) zb zb zb rs h (w) h (w) zb or

HgS

rh

HgSe HgTe

zb zb

2.6979 4.865 5.137 5.617 4.203 5.203 5.91 4.548 3.2495 3.8226 5.4102 5.6692 6.1037 4.686 4.1367 4.2999 6.481 3.577 (a) 8.681 (b) 2.427 (c) 0.745 (u) 4.14 (a) 9.49 (b) 2.292 (c) 0.720 (u) 0.480 (v) 6.084 6.4603

II–VI

c (A) 6.6612 4.982

5.1855

5.760

4.380

7.390 5.2069 6.2605

6.7161 7.0109

Table 1.5 Molecular weight M, lattice constant a and crystal density g for a number of cubic, diamondtype semiconductors at 300 K System

Material

M (amu)

a (A)

g (g/cm3)

IV

Diamond Si Ge Sn

12.0107 28.0855 72.61 118.710

3.5670 5.4310 5.6579 6.4892

3.5156 2.3291 5.3256 5.7710

Table 1.6 Molecular weight M, lattice constant a and crystal density g for a number of cubic, zincblende-type semiconductors at 300 K g (g/cm3)

40.0962

4.3596

3.2142

BN BP BAs AlN AlP AlAs AlSb GaN GaP GaAs GaSb InN InP InAs InSb

24.818 41.785 85.733 40.98828 57.955299 101.903098 148.742 83.730 100.696 144.645 191.483 128.825 145.792 189.740 236.578

3.6155 4.5383 4.777 4.38 5.4635 5.66139 6.1355 4.52 5.4508 5.65330 6.09593 4.986 5.8690 6.0583 6.47937

3.4880 2.9693 5.224 3.24 2.3604 3.73016 4.2775 6.02 4.1299 5.31749 5.61461 6.903 4.7902 5.6678 5.77677

BeO BeS BeSe BeTe MgO MgS MgSe MgTe ZnO ZnS ZnSe ZnTe CdO CdS CdSe CdTe HgS HgSe HgTe

25.0116 41.078 87.97 136.61 40.3044 56.371 103.27 151.91 81.39 97.46 144.35 192.99 128.410 144.477 191.37 240.01 232.66 279.55 328.19

3.80 4.865 5.137 5.617 4.21 5.62 5.91 6.42 4.47 5.4102 5.6692 6.1037 5.148a 5.825 6.077 6.481 5.8514 6.084 6.4603

3.03 2.370 4.310 5.120 3.59 2.11 3.32 3.81 6.05 4.0879 5.2621 5.6372 6.252a 4.855 5.664 5.856 7.7135 8.245 8.0849

Material

IV

3C-SiC

III–V

II–VI

a

Theoretical

a (A)

System

M (amu)

STRUCTURAL PROPERTIES

19

Table 1.7 Molecular weight M, lattice constants a and c and crystal density g for a number of hexagonal, wurtzite-type semiconductors at 300 K System

Material

a IV

2H-SiC

III–V

II–VI

a

g (g/cm3)

Lattice constant (A)

M (amu)

c

40.0962

3.0763

5.0480

3.2187

AlN GaN InN

40.98828 83.730 128.825

3.112 3.1896 3.548

4.982 5.1855 5.760

3.258 6.0865 6.813

BeO BeSa BeSea BeTea MgO MgS MgSe MgTe ZnO ZnS ZnSe ZnTe CdO a CdS CdSe CdTe HgS a HgSe a HgTe a

25.0116 41.078 87.97 136.61 40.3044 56.371 103.27 151.91 81.39 97.46 144.35 192.99 128.410 144.477 191.37 240.01 232.66 279.55 328.19

2.6979 3.440 3.632 3.972 3.199 3.972 4.145 4.548 3.2495 3.8226 3.996 4.27 3.678 4.1367 4.2999 4.57 4.1376 4.302 4.5681

4.380 5.618 5.932 6.486 5.086 6.443 6.723 7.390 5.2069 6.2605 6.626 6.99 5.825 6.7161 7.0109 7.47 6.7566 7.025 7.4597

3.009 2.370 4.311 5.120 2.970 2.127 3.429 3.811 5.6768 4.0855 5.232 5.81 6.249 4.8208 5.6615 5.90 7.7134 8.246 8.0850

Estimated or theoretical

1.4.3 Semiconductor Alloy (a) Group-IV semiconductor Table 1.8 gives the lattice-matching condition between some group-IV ternary alloys and Si substrate. The incorporation of carbon into Si or SiGe gives rise to additional flexibility for group-IV-based heterostructure design [11]. Due to huge lattice mismatch between diamond Table 1.8 Lattice-matching conditions of some group-IV ternaries at 300 K Material

Substrate

Expression

Remark

CxSiyGe1xy CxSiySn1xy CxGeySn1xy

Si Si Si

x ¼ 0.109–0.109y x ¼ 0.362–0.362y x ¼ 0.362–0.284y

0 y 1.0, x/(1 x y) ¼ 0.122 0 y 1.0, x/(1 x y) ¼ 0.567 0 y 0.89

20

PROPERTIES OF SEMICONDUCTOR ALLOYS

and Si, a small amount of substantially incorporated C induces a substantial tensile strain in pseudomorphic CxSi1x layers on Si. This effect can be exploited for CxSiyGe1xy/Si, CxSiySn1xy/Si and CxGeySn1xy/Si heterostructures by properly choosing pseudomorphic compositions x and y. It should be noted, however, that the solubility of C into Si is only about 6 106 at% (3 1017 cm3) at the melting point of Si. Carbon incorporated into substitutional lattice sites up to a few atomic percent has been achieved only using growth techniques far from thermodynamic equilibrium [12]. Figure 1.6 shows the plot of the lattice constant a versus x for bulk CxSi1x. The open circles represent the experimental data for diamond and Si, while the solid circle shows the data for 6.0

a (Å)

5.5

CxSi1-x

5.0 4.5 4.0 3C-SiC

3.5 3.0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.6 Lattice constant a versus x for bulk CxSi1x at 300 K. The open and solid circles represent the experimental data. The light solid and dashed lines represent the results of Vegard law between Si (x ¼ 0) and 3C-SiC (x ¼ 0.5) and between Si (x ¼ 0) and diamond (x ¼ 1.0), respectively. The heavy solid line shows the theoretical values obtained from a Monte Carlo simulation by Kelires [13]

3C-SiC (x ¼ 0.5). The light solid line is obtained from Vegard law between Si and 3C-SiC (x ¼ 0.5), while the dashed line is obtained between Si and diamond (x ¼ 1.0). The 3C-SiC value is smaller than the linearly interpolated value. The heavy solid line in Figure 1.6 represents the theoretical a values for C xSi1x obtained from a Monte Carlo calculation [13]. These values can be expressed as (in A) aðxÞ ¼ 5:43102:4239x þ 0:5705x2

ð1:3Þ

The negative deviation a(x) seen in Figure 1.6 has been confirmed experimentally from pseudomorphic CxSi1x epilayers (x < 0.012) grown on Si(100) by solid-source MBE [14]. Si and Ge, both crystallize in the diamond structure, form a continuous series of SixGe1x alloys with x ranging from 0 to 1.0. The most precise and comprehensive determination of the lattice constant a and crystal density g across the whole alloy range was undertaken by Dismukes et al. [15]. The values they obtained for a and g are plotted versus x for SixGe1x in Figure 1.7. These data reveal a small deviation from Vegard law, i.e. from the linearity between the endpoint values. The lattice parameter a shows a downward bowing, while the density parameter g gives an upward bowing. From Figure 1.7, we obtain parabolic relation for a and g as a function of x (a in A, g in g/cm3) aðxÞ ¼ 5:65750:2530x þ 0:0266x2

ð1:4aÞ

gðxÞ ¼ 5:32562:5083x0:4853x2

ð1:4bÞ

STRUCTURAL PROPERTIES

21

5.7 a (Å)

(a) 5.6 5.5

SixGe1-x

g (g/cm3)

5.4 6 (b)

5 4 3 2

0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.7 (a) Lattice constant a and (b) crystal density g for SixGe1x at 300 K. The experimental data are taken from Dismukes et al. [15]. The solid and dashed lines represent the parabolic and linear fit results, respectively

As shown in Figure 1.8, the diamond-type lattice, e.g. Si has only one type of first-neighbor distance pﬃﬃﬃ 3 a ðfour bondsÞ ð1:5Þ dðSiSiÞ ¼ 4 EXAFS has been popularly used to determine bond lengths for different types of neighbor atom pairs and the corresponding fractional occupancy of each type of neighbor. Recent EXAFS and XRD studies performed on strained SixGe1x/Si layers indicated that the Si–Si, Si–Ge and Ge–Ge nearest-neighbor distances are 2.35 0.02, 2.42 0.02 and 2.38 0.02 A, respectively, close to the sum of their constituent-element covalent radii and independent of x, while the lattice constant varies monotonically with x [16,17]. More recently, Yonenaga et al. [18] investigated the local atomistic structure in bulk Czochralski-grown SixGe1x using EXAFS. As shown in Figure 1.9, the bond lengths Si–Si, Si–Ge and Ge–Ge in the bulk SixGe1x remain distinctly different lengths and vary in linear fashion of x over the entire composition range 0 x 1.0, in agreement with expectation derived from ab-initio electronic structure calculation. These results suggest that SixGe1x is a typical disorder material and that the bond lengths and bond angles are disordered with x in SixGe1x.

Figure 1.8 Bond distances in (a) diamond (Si), (b) zinc-blende (GaAs) and (c) wurtzite structures (GaN)

22

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 1.9 Near-neighbor distance in SixGe1x at 300 K. The experimental data are taken from Yonenaga et al. [18]. The horizontal lines show the bond lengths in bulk Si and Ge. The middle thin line is obtained from Vegard law

(b) III–V semiconductor The expressions for a versus alloy composition can be obtained from Vegard law. The crystal density can also be calculated from g ¼ MdM/NA, where M is the molecular weight, NA ¼ 6.022 1023 mol1 is the Avogadro constant and dM is the molecular density [1]. The III–V quaternaries can be epitaxially grown on some III–V binaries (GaAs, InP, etc.). Introducing the binary lattice parameters in Table 1.6 into Equation (A.6) or Equation (A.8), we can obtain the lattice-matching conditions for AxB1xCyD1y and AxByC1xyD quaternaries on various III–V binary substrates. These results are summarized in Tables 1.9–1.11. The lattice-matching conditions in Tables 1.9–1.11 can be approximated by more simple expressions. Some results are presented in Table 1.12. The lattice parameter a at 300 K as a function of x for AlxGa1xAs is shown in Figure 1.10. The experimental data are taken from Takahashi [19]. From a least-squares fit, we obtain aðxÞ ¼ 5:6533 þ 0:0083x0:0003x2

ð1:6Þ

The solid line in Figure 1.10 shows the calculated result of Equation (1.6). This equation promises that the lattice parameter for AlxGa1xAs can be given by Vegard law with good Table 1.9 Lattice-matching conditions for some cubic, zinc-blende-type III–V quaternaries of type AxB1xCyD1y at 300 K x¼

A0 þ B0 y C0 þ D0 y

Quaternary

Substrate

A0

B0

C0

D0

AlxIn1xPyAs1y

GaAs InP GaAs InP

0.4050 0.1893 0.4050 0.1893

0.1893 0.1893 0.1893 0.1893

0.3969 0.3969 0.4050 0.4050

0.0086 0.0086 0.0132 0.0132

GaxIn1xPyAs1y

Remark 0.04y1.0 0y1.0 0y1.0 0y1.0

STRUCTURAL PROPERTIES

23

Table 1.10 Lattice-matching conditions for some cubic, zinc-blende-type III–V quaternaries of type AxB1xCyD1y at 300 K y¼

A0 þ B0 x C0 þ D0 x

Quaternary

Substrate

A0

B0

C0

D0

AlxGa1xPyAs1y AlxGa1xPySb1y

GaAs GaAs GaSb InP InAs GaSb InP InAs GaAs GaSb InP InAs GaSb InP InAs GaAs GaSb InP InAs GaSb InP InAs

0 0.4426 0 0.2269 0.0376 0 0.2269 0.0376 0.8261 0.3834 0.6104 0.4211 0.3834 0.6104 0.4211 0.8261 0.3834 0.6104 0.4211 0.3834 0.6104 0.4211

0.0081 0.0396 0.0396 0.0396 0.0396 0.0396 0.0396 0.0396 0.3439 0.3439 0.3439 0.3439 0.3439 0.3439 0.3439 0.3834 0.3834 0.3834 0.3834 0.3834 0.3834 0.3834

0.2025 0.6451 0.6451 0.6451 0.6451 0.4426 0.4426 0.4426 0.6104 0.6104 0.6104 0.6104 0.4211 0.4211 0.4211 0.6104 0.6104 0.6104 0.6104 0.4211 0.4211 0.4211

0.0046 0.0269 0.0269 0.0269 0.0269 0.0315 0.0315 0.0315 0.0616 0.0616 0.0616 0.0616 0.0530 0.0530 0.0530 0.0348 0.0348 0.0348 0.0348 0.0216 0.0216 0.0216

AlxGa1xAsySb1y AlxIn1xPySb1y

AlxIn1xAsySb1y GaxIn1xPySb1y

GaxIn1xAsySb1y

Remark 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0.53 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0.48 x 1.0 0 x 1.0 0.52 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0.47 x 1.0 0 x 1.0

Table 1.11 Lattice-matching conditions for some cubic, zinc-blende-type III–V quaternaries of the type AxByC1xyD or ABxCyD1xy at 300 K Quaternary

Substrate

Expression

Remark

AlxGayIn1xyP AlxGayIn1xyAs AlPxAsySb1xy

GaAs InP GaAs InP InAs GaAs InP InAs GaSb InAs

y ¼ 0.5158–0.9696x y ¼ 0.4674–0.9800x x ¼ 0.7176–0.7055y x ¼ 0.3966–0.7055y x ¼ 0.1149–0.7055y x ¼ 0.6861–0.6861y x ¼ 0.3518–0.6861y x ¼ 0.0583–0.6861y x ¼ 0.6282–0.6899y x ¼ 0.6899–0.6899y

0 x 0.53 0 x 0.48 0 y 1.0 0 y 0.56 0 y 0.16 0 y 1.0 0 y 0.51 0 y 0.08 0 y 0.91 0 y 1.0

GaPxAsySb1xy InPxAsySb1xy

24

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.12 Approximated lattice-matching expression for some important cubic, zinc-blende-type III–V quaternaries at 300 K Quaternary

Substrate

Expression

Remark

AlxGa1xAsySb1y

GaSb InAs InP GaSb InAs GaAs InP

y ¼ 0.084x y ¼ 0.085 þ 0.078x x ¼ 0.47–0.47y y ¼ 0.91–0.91x y ¼ 1.00–0.91x y ¼ 0.52–0.97x y ¼ 0.47–0.98x

0 x 1.0 0 x 1.0 0 y 1.0 0 x 1.0 0 x 1.0 0 x 0.53 0 x 0.48

GaxIn1xPyAs1y GaxIn1xAsySb1y AlxGayIn1xyP AlxGayIn1xyAs

5.665 AlxGa1-xAs a (Å)

5.660

5.655

5.650 0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.10 Lattice parameter a as a function of x for AlxGa1xAs at 300 K. The experimental data are taken from Takahashi [19]. The solid line represents the quadratic least-squares fit

approximation. The difference in a between AlxGa1xAs and GaAs can also be written as aðAlx Ga1x AsÞaðGaAsÞ ¼ 0:0015x ¼ 0:15x% aðGaAsÞ

ð1:7Þ

Figure 1.11 shows the experimental x–y plots for GaxIn1xPyAs1y/InP [20]. The solid line shows the exactly calculated x–y relation in Table 1.9 1.0 Ga x In1-xPyAs1-y /InP

0.8 y

0.6 0.4 Exact Approx.

0.2 0

0

0.1

0.2

0.3

0.4

0.5

x

Figure 1.11 Plots of x versus y for GaxIn1xPyAs1y nearly lattice-matched to InP at 300 K. The experimental data are taken from Nahory et al. [20]. The solid and dashed lines show the lattice-matching relationships obtained from Vegard law in Equations (1.8) and (1.9), respectively

STRUCTURAL PROPERTIES

x¼

0:18930:1893y 0:4050 þ 0:0132y

25

ð1:8Þ

The dashed line also shows the calculated result using an expression in Table 1.12 x ¼ 0:470:47y

ð1:9Þ

Both expressions can explain the experimental x–y relation very well and simultaneously indicate the validity of Vegard law for GaxIn1xPyAs1y/InP. It has, however, been reported that strained AlxGa1xSb/GaSb does not obey Vegard law [21]. The crystal density g versus y for GaxIn1xPyAs1y/InP is shown in Figure 1.12. The solid line represents the X-ray crystal density calculated from Equation (1.16) of Adachi [1], while the dashed line is obtained from the linear interpolation between the endpoint densities (y ¼ 0, 1.0). Their difference is within 2%. 6.0 GaxIn1-xPyAs1-y/InP

g (g/cm-3)

5.5 5.0

Exact Approx.

4.5 4.0 0

0.2

0.4

0.6

0.8

1.0

y

Figure 1.12 X-ray crystal density g versus y for GaxIn1xPyAs1y/InP at 300 K. The solid line represents the exact X-ray crystal density calculated from Equation (1.16) of Adachi [1], while the dashed line is obtained from the linear interpolation between the endpoint binary data

The experimental lattice parameter c as a function of x for w-GaxIn1xN is plotted in Figure 1.13. The experimental data are taken from Bearch et al. [22] (solid circles) and Romano et al. [23] (open circles). The GaxIn1xN layers (0 x 0.14) used by Bearch et al. [22] were grown on (0001) sapphire by MOMBE and were believed to be fully relaxed. On the other hand, the GaxIn1xN layers in Romano et al. [23] were pseudomorphically grown on 5 mm thick GaN on (0001) sapphire by MOCVD (x ¼ 0–0.114). The solid line in Figure 1.13 obeys Vegard law using c ¼ 5.1855 A for GaN and c ¼ 5.760 A for InN (Table 1.7). Figure 1.14 shows the lattice parameter c versus x for strained AlxGa0.9xIn0.1N alloy grown by MOCVD [24]. The dashed line represents the linear interpolation result using the endpoint values taken from Table 1.7. The lattice parameter c is found to decrease almost linearly with increasing x. The prediction of Vegard law gives no good agreement with the experimental data. It can be concluded from Figure 1.13 that the fully relaxed GaxIn1xN films follow Vegard law well; however, no good agreement can be achieved in the case of the pseudomorphic alloy layers. As we will see later (Section 1.5.2), Vegard law may be applicable if any strain effects are artificially removed from such pseudomorphically strained layers. HRXRD has been widely used and demonstrated that almost all III–V semiconductor alloys obey Vegard law well. It has also been reported that Vegard law remains valid in dilute nitrides, such as GaNxAs1x and GaxIn1xNyAs1y, as long as all N atoms in the dilute nitrides locate at the arsenic sites [25]. The N–N pairs are thought to be the predominant N-related defects that cause deviation from Vegard law [26]. Germini et al. [21], however, observed a deviation

26

PROPERTIES OF SEMICONDUCTOR ALLOYS 5.30

c (Å)

5.28

w-GaxIn1-xN

5.26 5.24 5.22 5.20 5.18 0.80

Vegard law

0.85

0.90 x

0.95

1.00

Figure 1.13 Lattice parameter c as a function of x for w-GaxIn1xN at 300 K. The experimental data are taken from Bearch et al. [22] (fully relaxed layers, solid circles) and Romano et al. [23] (pseudomorphic layers, open circles). The solid line represents the simply estimate of the c versus x relationship obtained from Vegard law 5.30

c (Å)

5.25

w-AlxGa0.9-xIn0.1N

5.20 5.15 5.10 0

Vegard law

0.05 0.10 0.15 0.20 0.25 0.30 x

Figure 1.14 Lattice parameter c versus x for strained w-AlxGa0.9xIn0.1N at 300 K. The experimental data are taken from Aumer et al. [24]. The dashed and solid lines represent the results of applying Vegard law before and after correcting for the biaxial strain effect

from Vegard law in MBE-grown AlxGa1xSb/GaSb layers by HRXRD, RBS and RHEED. These results are plotted in Figure 1.15. The experimental unstrained lattice parameters can be described by aðxÞ ¼ 6:09593 þ 0:04360x4:229 103 x2

ð1:10Þ

The deviation from linearity is found to be larger than the prediction of a perfect random alloy in the frame of the Fournet model [27]. There is a significant structural difference between the bond distance in the zinc-blende and wurtzite structures of AxB1xC alloy. The first-neighbor distance in the zinc-blende structure is given from Figure 1.8 by pﬃﬃﬃ 3 dðGaAsÞ ¼ a ðfour bondsÞ ð1:11Þ 4 Yet, the wurtzite structure has two types of the first-neighbor anion–cation bond distances (Figure 1.8) dðGaN1 Þ ¼ ua ðone bondÞ

ð1:12aÞ

STRUCTURAL PROPERTIES

27

6.140 Al xGa 1-x Sb

a (Å )

6.130 6.120 6.110 6.100 6.090

0

0. 2

0. 4

0. 6

0. 8

1. 0

x

Figure 1.15 Room-temperature lattice constant a as a function of x for AlxGa1xSb grown on GaSb. The experimental data are taken from Germini et al. [21]. The solid line represents the quadratic best-fit result obtained using Equation (1.10)

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 1 1 c þ u aw ðthree bondsÞ dðGaN2 Þ ¼ 3 2 aw

ð1:12bÞ

where u represents the cell-internal structural parameter and aw and c show the lengths of the lattice vectors of the wurtzite structure. In the case of an ideal tetragonal ratio c/aw ¼ (8/3)1/2 ¼ 1.6330 and an ideal cell internal parameter u ¼ 3/8, it follows from Equation (1.12) that d(Ga–N1) ¼ d(Ga–N2). In the zinc-blende lattice, we have only one type of second neighbor cation–anion bond distance pﬃﬃﬃﬃﬃ 11 a ð12 bondsÞ ð1:13Þ dðGaAsÞ ¼ 4 On the other hand, the wurtzite lattice has three types of second neighbor cation–anion distances concerning the cation A (Ga) to anions C2a, C2b and C2c c dðGaN2a Þ ¼ ð1uÞ aw ðone bondÞ ð1:14aÞ aw sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 uc aw ðsix bondsÞ dðGaN2b Þ ¼ 1 þ ð1:14bÞ aw sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 4 1 c þ u aw ðthree bondsÞ ð1:14cÞ dðGaN2c Þ ¼ 3 2 aw For ideal wurtzite parameters of c/aw ¼ (8/3)1/2 ¼ 1.6330 and u ¼ 3/8, the following expression can be obtained from Equation (1.14) dðGaN2a Þ ¼ 1:0206aw ; dðGaN2b Þ ¼ dðGaN2c Þ ¼ 1:1726aw

ð1:15Þ

The spacing between the near-neighbor In–In or P–P atoms in InP is equal to (1/H2)a. It would be anticipated that for an alloy the interatomic bond length of each constituent remains constant with alloy composition. Unfortunately, however, standard XRD techniques give information only on the lattice structure that is averaged over an area larger than the scale of

28

PROPERTIES OF SEMICONDUCTOR ALLOYS

lattice constant. The interatomic structure in such semiconductor alloys was, therefore, not well understood until 1982. Mikkelsen and Boyce [28] reported in 1982 the interatomic structure of GaxIn1x As using an EXAFS. They found that the Ga–As and In–As near-neighbor distances change by only 0.04 A as the In composition varies from 1 to 99 at% despite the fact that this alloy accurately follows Vegard law with a change in average near-neighbor spacing of 0.17 A. We reproduce in Figure 1.16 the results of Mikkelsen and Boyce [28]. They also observed that the cation sublattice approaches a virtual crystal (i.e. an average fcc lattice) with a broadened single distribution of second-neighbor distances, whereas the anion sublattice exhibits a bimodal anion–anion second-neighbor distribution.

Figure 1.16 Near-neighbor distance in GaxIn1xAs at 300 K. The middle thin line represents the bond length curve estimated from Vegard law. [Reprinted with permission from J. C. Mikkelsen, Jr. and J. B. Boyce, Phys. Rev. Lett. 49, 1412 (1982). Copyright (1982) by the American Physical Society]

The essentially same EXAFS results, but on GaxIn1xPyAs1y/InP, were reported by Oyanagi et al. [29]. They reported that the cation–anion distances in GaxIn1xPyAs1y/InP deviate from the average interatomic distance, but are rather close to the bond lengths in pure parent crystals. The cation–anion distances obtained from this study are plotted in Figure 1.17. The near-neighbor distances in w-GaxIn1xN versus x are shown in Figure 1.18. The experimental data are taken from Jeffe et al. [30]. The theoretical lines are taken from Mattila and Zunger [31] in which the valence force field simulation with large supercells (512–1280 atoms) was used. It has been shown [31] that while the first-neighbor cation–anion bonds for different cations (Ga–N1 and In–N1) retain distinct values in the wurtzite and zinc-blende alloys, the second-neighbor cation–anion bonds Ga–N2 and In–N2 merge into a single bond length. However, the second-neighbor cation–anion bonds for the same cation exhibit a crucial difference between the wurtzite and zinc-blende structures. This is thought to be an intrinsic property of the binary constituents and persists in the alloy. The small splitting of the firstneighbor cation–anion bonds in the wurtzite structure is also preserved in the alloy, but obscured by bond length broadening [31].

STRUCTURAL PROPERTIES

29

Near-neighbor distance (Å)

2.70 2.65 2.60

Gax In1-x Py As1-y /InP In-As

2.55 Vegard law

2.50 2.45

Ga-As

2.40

Ga-P

2.35 2.30 0

0.2

0.4

0.6

0.8

1.0

y

Figure 1.17 Near-neighbor distance in GaxIn1xPyAs1y/InP at 300 K. The experimental data are taken from Oyanagi et al. [29]. The dashed line represents the bond length curve obtained from Vegard law

Figure 1.18 Near-neighbor distances versus x for w-GaxIn1xN. The experimental data were measured at 300 K by Jeffe et al. [30]. The theoretically calculated lines are taken from Mattila and Zunger [31] who used the valence force field simulation with large supercells (512–1280 atoms)

(c) II–VI semiconductor Several II–VI semiconductor quaternaries can be epitaxially grown on III–V binary substrates. The corresponding lattice-matching relationships are shown in Tables 1.13 and 1.14. These relationships can be approximated using more simple expressions, as listed in Table 1.15. Figure 1.19 shows the lattice constant a as a function of x for ZnxCd1xTe. The experimental data were obtained at 300 K using an XRD combined with a WDXS [32]. The combination with WDXS led to an absolute composition error Dx of less than 0.01. These data suggest that Vegard

30

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.13 Lattice-matching conditions for some cubic, zinc-blende-type II–VI quaternaries of the type AxB1xCyD1y at 300 K y¼

A0 þ B0 x C0 þ D0 x

Quaternary

Substrate

A0

B0

C0

D0

Remark

MgxZn1xSySe1y MgxZn1xSeyTe1y

GaAs InP

0.016 0.235

0.241 0.314

0.259 0.435

0.031 0.075

0 x 1.0 0 x 0.84

Table 1.14 Lattice-matching conditions for some cubic, zinc-blende-type II–VI quaternaries of the type AxByC1xyD at 300 K Quaternary

Substrate

Expression

Remark

BexMgyZn1xySe MgxZnyCd1xySe

GaAs InP

x ¼ 0.030 þ 0.453y y ¼ 0.510–0.409x

0 y 0.67 0 x 0.83

Table 1.15 Approximated lattice-matching expression for some important cubic, zinc-blende-type II–VI quaternaries at 300 K Quaternary

Substrate

Expression

Remark

MgxZn1xSySe1y MgxZn1xSeyTe1y BexMgyZn1xySe MgxZnyCd1xySe

GaAs InP GaAs InP

y ¼ 0.08 þ 0.82x y ¼ 0.55 þ 0.54x x ¼ 0.03 þ 0.45y y ¼ 0.51–0.41x

0 x 1.0 0 x 0.84 0 y 0.67 0 x 0.83

law is exactly valid within the limits of error Da/a 4 104 and follows the equation (in A) aðxÞ ¼ 6:48220:3792x

ð1:16Þ

CdSxTe1x shows a zinc-blende–wurtzite crystalline phase change at any alloy composition. Early studies failed to grow alloys for the full range of compositions, concluding that a large 6.6

a (Å)

6.5

ZnxCd1-xTe

6.4 6.3 6.2 6.1 6.0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.19 Lattice constant a as a function of x for ZnxCd1xTe at 300 K. The experimental data are taken from Schenk et al. [32]. The solid line represents the linear best fit of Equation (1.16)

STRUCTURAL PROPERTIES

31

miscibility gap exists in the CdS–CdTe pseudobinary system [33]. In 1973 Ohata et al. [34] studied the bulk alloy system for the full range of compositions and reported a change in the crystalline phase at x 0.2. Figure 1.20 plots the lattice constants a and c versus x for bulk CdSxTe1x crystals as measured by Wood et al. [35] using XRD. The composition x of each pellet was determined independently using PIXE. In Figure 1.20, the phase change occurs at x 0.2, in agreement with Ohata et al. [34]. The solid triangles represent the effective cubic lattice parameters aeff ¼ (H3a2c)1/3 defined in Adachi [1]. It can be concluded from Figure 1.20 that the lattice parameters both in the zinc-blende and wurtzite phases obey Vegard law well. It is also understood that if we consider aeff, instead of a or c, in the wurtzite phase (0.2 < x 1.0), CdSxTe1x gives the linear relationship between a and x over the whole alloy range (0 x 1.0). 8 c (w)

a (Å)

7 a (zb) 6 CdSxTe1-x

5

a (w)

4 0

0.2

0.4

x

0.6

0.8

1.0

Figure 1.20 Lattice constants a and c versus x for bulk CdSxTe1x in the zinc-blende (zb) and wurtzite (w) structures at 300 K. The experimental data are taken from Wood et al. [35]. The solid triangles represent the effective cubic parameters aeff ¼ (H3a2c)1/3

Near-neighbor distance (Å)

Motta et al. [36] carried out EXAFS measurements on ZnxCd1xTe. These results are shown in Figure 1.21 by the open circles. The solid circles correspond to the XRD data by Schenk et al. [32]. We can see that the EXAFS bond lengths in Figure 1.21 change much less than the nearest-neighbor distances determined from the XRD. As in the case of the III–Valloys (Figures 1.16 and 1.17), the XRD lattice parameters in II–VI alloys do not reflect the actual bond lengths of the nearest neighbors. The EXAFS data of Motta et al. [36] agreed with a random distribution of atoms in the mixed cation sublattice. 2.85 ZnxCd1-xTe

2.80 2.75

Cd-Te

2.70

Zn-Te

2.65 2.60

0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.21 Near-neighbor distance in ZnxCd1xTe at 300 K. The experimental data (open circles) are taken from Motta et al. [36]. The solid circles represent the bond lengths obtained from the XRD data by Schenk et al. [32]

32

PROPERTIES OF SEMICONDUCTOR ALLOYS

1.5 COHERENT EPITAXY AND STRAIN PROBLEM 1.5.1 Bilayer Model Recent semiconductor devices usually have multilayer structures. The distribution of strains in multilayer structures is the subject of perennial, great interest since internal strains normally arise in thin epitaxial films during the preparation by heteroepitaxial growth. Internal strains or stresses are a consequence of the mismatch of lattice constants and/or the difference in the thermal expansion coefficients of the individual layers. The strain and stress are related through the fourth-rank elastic stiffness [C] or compliance tensor [S] [1]. Let us consider the case of bonding a thin plate of zinc-blende crystal of size Neae Neae te onto a substrate of a different size Nsas Nsas ts, where Ni is the number of lattice atoms along the edge of the crystal plate, ai is the lattice constant and ti is the thickness of the plate; see Figure 1.22(a) [37]. To achieve a coherent interface, Ne is set to equal Ns. Let us assume that ae is less than as and thus le ¼ Neae is less than ls ¼ Nsas. The bonding operation is carried out in the following manner: equal and opposite forces F are applied to the plates to stretch plate ‘e’ and compress plate ‘s’ uniformly in the lateral direction to the same final dimension lf lf. The two plates are then bonded together with a perfect alignment of the atomic planes; see Figure 1.22(b). At the moment when the two plates are bonded together, the composite experiences an applied bending moment given by F(ts þ te)/2, which is counterbalanced by the moment resulting from the internal elastic stress. Finally, the applied forces are relieved, and the moments from the elastic stresses bend the composite in the direction shown in

Figure 1.22 Formation of a two-layer composite: (a) two single-crystalline plates with the lattice constants ae and as (ae < as) and thicknesses te and te, respectively; (b) layer ‘e’ is stretched and layer ‘s’ is compressed to match the macroscopic dimension, and the two layers are then bonded together to form a composite; (c) the composite bends toward the side with the shorter lattice constant after removal of the external stresses Fe and Fs

STRUCTURAL PROPERTIES

33

Figure 1.22(c). The bending of the composite relaxes some of the stress, and the radius of curvature is determined by the final state of the internal stress. Based on this bilayer model, Noyan and Segm€ uller [37] obtained the coherency condition in terms of the curvature radius R 3 ae as 2 ts ae te 1 ae a s Ee t e Es t s Ee ts2 te 1þ þ ¼ 1þ þ R 4 Ee ts te ð1 þ te =ts Þ as as as ts a e Es t s 12 4

ð1:17Þ

where Ei ¼

Yi 1Pi

ð1:18Þ

with Y ¼ Young’s modulus and P ¼ Poisson’s ratio. The term d shown in Figure 1.22(c) represents the shift of the neutral axis of the composite from ts/2. This quantity is given by d¼

te Ee 1 þ te =ts 2Es 1 þ ðEe te =Es ts Þ

ð1:19Þ

Solving the elastic force and momentum balance equations, Noyan and Segm€uller [37] gave the elastic stress component Xxx parallel to the film as e Xxx ¼

Ee as ae as ae te ts 1þ 1 þ ðas Ee te =ae Es ts Þ ae as as ts 2R

ð1:20Þ

The relationship between the film and substrate stresses is given by te e s ¼ Xxx Xxx ts

ð1:21Þ

The dependence of Xxx on z is now given by e e Xxx ðzÞ ¼ Xxx þ Ee

s e Xxx ðzÞ ¼ Xxx

zte =2 R

for

te z þ te =2 þ Es R ts

0 z te

ð1:22aÞ

for

ð1:22bÞ

0 z ts

s e < 0; Xxx > 0, and R < 0. In the case where ae < as, these expressions give Xxx

1.5.2 Elastic Strain and Lattice Deformation Since Xzz is equal to zero in the bilayer model discussed above, the lattices are free to expand or contract in the z direction, that is, perpendicular to the interface. As seen in Figure 1.23, this i i causes the cubic lattice structure to be tetragonally distorted. Since both Xxx and Xyy have opposite signs for i ¼ s compared to i ¼ e, the two cubic lattices are tetragonally distorted in the opposite sense, one with the lattice constant perpendicular to the interface lengthened and

34

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 1.23 Cross section of an ‘epilayer–substrate’ system, where ae and as are the unstrained lattice parameters of the epilayer and substrate, respectively

the other shortened. Therefore, the measured vertical mismatch is enhanced by the tetragonal distortion. Lattice deformation between the epilayer and substrate can be determined by conventional XRD. For example GaxIn1xPyAs1y epilayers on InP(100) are shown in Figure 1.24 [38], where the GaxIn1xPyAs1y/InP samples were grown by LPE with the Ga atomic fractions in liquid solution between 0.4 an 1.0 at%. The experimental lattice deformation Da/a perpendicular to the layer surface for layers with a Ga fraction lower than 0.0065 has a positive value (i.e. compressive strain in the growth direction), while it has negative values (tensile strain) for layers with a fraction larger than 0.0065. In practical cases where the thickness of the epilayer is very small compared to that of the substrate, the lattice mismatch can be taken up totally by the tensile or compressive strain inside the epilayer, giving a coherent interface. A discontinuity in the lattice constant parallel to the interface can exist only in the presence of misfit dislocations. Nagai [39] studied the

Figure 1.24 Lattice mismatch in a GaInPAs/InP heterostructure as a function of the Ga atom fraction in LPE-growth liquid solution. [Reprinted with permission from K. Oe and K. Sugiyama, Appl. Phys. Lett. 33, 449 (1978). Copyright (1978) by the American Institute of Physics]

STRUCTURAL PROPERTIES

35

effects of lattice misfit on the lattice deformation for GaxIn1xAs on GaAs by HT-VPE. The thickness of the substrates was in the range 2–5 mm and the epilayer was in the range 5–10 mm. His results are shown in Figure 1.25, where a|| is the unstrained lattice parameter of the substrate (GaAs) and a? is the strained lattice parameter of the epilayer due to tetragonal distortion.

Figure 1.25 Lattice-constant ratio ae/as for HT-VPE-grown GaxIn1xAs on (1 0 0) and (1 1 1)As planes of GaAs. [Reprinted with permission from H. Nagai, J. Appl. Phys. 45, 3789 (1974). Copyright (1974) by the American Institute of Physics]

The lattice constant of InAs (6.0583 A) is larger than that of GaAs (5.65330 A). Thus, the GaxIn1xAs lattice on GaAs is expected to be tetragonally distorted with the lattice constant perpendicular to the interface being lengthened. The measured lattice constants perpendicular to the film are indeed larger than that along the surface. In the region x > 0.8 the degree of deformation increased with decreasing x, but in the region x < 0.8 it decreased with decreasing x. With the aid of defect revealing etching, it was concluded that in the region x > 0.8 the lattice mismatch is relieved only by tetragonal distortion and for x < 0.8 it is relieved by both misfit dislocation and tetragonal distortion. Figure 1.26 plots the lattice constant a versus x for strained CxSi1x alloy grown on Si(100) by solid-source MBE. The experimental data are taken from Berti et al. [14]. The dash-dotted

a⊥ (Å)

5.44

5.42

CxSi1-x

5.40

5.38 0

0.004 0.008 0.012 0.016 0.020 x

Figure 1.26 Lattice constant a versus x for strained CxSi1x grown on Si(1 0 0) by solid-source MBE. The experimental data are taken from Berti et al. [14]. The dash-dotted line represents the linearly interpolated values between diamond and Si. The light solid and dashed lines are calculated from Equation (1.23) by introducing a0 values estimated from Vegard law between Si and 3C-SiC (x ¼ 0.5) and between Si and C (x ¼ 1.0), respectively. The heavy solid line is calculated by introducing the Monte Carlo-simulated lattice constants reported by Kelires [13] as a0

36

PROPERTIES OF SEMICONDUCTOR ALLOYS

line shows the linear interpolation result between diamond (a ¼ 3.5670 A) and Si (a ¼ 5.4310 A). We can see that the linear interpolation scheme predicts quite different lattice parameters from the experimental data. The strain in the epilayer and hence the lattice constant in growth direction a? can be calculated from the elastic theory [37] 2P a? ¼ ða0 ajj Þ 1 þ ð1:23Þ þ ajj 1P where a0 is the lattice constant of the relaxed material, a|| is the in-plane lattice constant assumed to be the same as the substrate parameter and P is Poisson’s ratio. In the case of cubic materials, Equation (1.23) can be rewritten as 2C12 a? ¼ ða0 ajj Þ 1 þ ð1:24Þ þ ajj C11 where Cij is the elastic stiffness constant. The light solid and dashed lines in Figure 1.26 represent the calculated results of Equation (1.23) by introducing a0 values estimated from Vegard law between Si and 3C-SiC (x ¼ 0.5) and between Si and diamond (x ¼ 1.0), respectively (Figure 1.6). The heavy solid line is also obtained from Equation (1.23) by introducing Monte Carlo-simulated lattice constants [13] as a0. The P values in Equation (1.23) are obtained from the linear interpolation between diamond and Si [1]. The results in Figure 1.26 suggest that the lattice constant a in CxSi1x significantly deviates from Vegard law. The relationship between a and x can be finally given by Equation (1.3). Figure 1.27 shows the lattice parameters perpendicular and parallel to the epilayer surface of MOMBE-grown GaNxAs1x on GaAs(100) [40]. The experimental data clearly suggest that the GaNxAs1x layers are coherently grown on the GaAs(100) substrates. The dashed line is simply estimated from the linear interpolation between c-GaN and GaAs. The solid lines are calculated from Equation (1.23) with a|| ¼ 5.6517 A. The relaxed parameter a0 and Poisson’s ratios used in the calculation are taken from Vegard law between c-GaN and GaAs [1]. We can see in Figure 1.27 excellent agreement between the calculated and experimental lattice parameters.

5.70 a||

a (Å)

5.65 5.60 5.55

a⊥

GaNxAs1-x Vegard law

5.50 0

0.01

0.02

0.03

0.04

0.05

x

Figure 1.27 Lattice parameters perpendicular (a?) and parallel (a||) to the epilayer surface of MOMBEgrown dilute-nitride GaNxAs1x on GaAs(1 0 0). The experimental data are taken from Uesugi et al. [40]. The dashed line is simply estimated from Vegard law between c-GaN and GaAs. The solid lines are calculated from Equation (1.23) with a|| ¼ 5.6517 A (const.). The relaxed parameters a0 and Poisson’s ratios P are taken from Vegard law between c-GaN and GaAs

STRUCTURAL PROPERTIES

37

The essentially same analysis as in Figure 1.27 is performed on strained AlxGa0.9xIn0.1N grown by MOCVD [24]. The solid line in Figure 1.14 represents the result of this analysis. Note that Poisson’s ratio is a crystallographic plane- and direction-dependent quantity. The expressions of Poisson’s ratio P and corresponding numeric values for some hexagonal semiconductors are summarized in Tables 3.19 and 3.20 of Adachi [1]. The quaternary P values used in Equation (1.23) are estimated from Vegard law. The in-plane lattice constant a|| is assumed to be 5.240 A. In Figure 1.14, there is good agreement between the calculated and experimental values even in the wurtzite crystal structure. However, in the case of relaxed AlxIn1xN alloy Vegrad law leads to an overestimation of the In mole fraction, which cannot be explained by either strain state or impurity levels. The In atomic fraction can be overestimated by as much as 6–37% in the range of 0.18 < x < 0.93 [41]. Figures 1.28(a) and 1.28(b) show the experimental lattice parameters a and c for MgxZn1xO layers on sapphire (0001) [42] and on 6H-SiC (0001) [43]. The solid lines show the linear interpolation results of c and a between MgO and ZnO. The effective cubic lattice parameters aeff ¼ (H3a2c)1/3 for MgO and ZnO are, respectively, 4.484 and 4.567 A, while those for sapphire and 6H-SiC are 6.335 A and 4.359 A, respectively. Coherently grown MgxZn1xO films on the sapphire and 6H-SiC substrates will be tensile- and compressive-strained, respectively. The ZnO (x ¼ 0) layers, however, exhibited virtually relaxed lattice constants of 3.246 and 5.205 A along the a and c axes, respectively. As seen in Figure 1.28, the c- (a-) axis length decreased (increased) with increasing x for MgxZn1xO both on the sapphire and 6H-SiC substrates. The resulting ratio c/a decreased with increasing x, indicating that the MgxZn1xO films are considerably distorted from the ideal wurtzite although they are in the relaxed states.

Figure 1.28 (a) a-axis and (b) c-axis lattice parameters at 300 K for MgxZn1xO grown on Al2O3 (0001) substrate by Ohtomo et al. [42] and on 6H-SiC (0001) substrate by Ashrafi and Segawa [43]. The solid lines in (a) and (b) show the linearly interpolated values of a and c between MgO and ZnO. The corresponding c/a ratios are plotted in (c)

1.5.3 Critical Thickness Pseudomorphic epitaxy, in which a high-quality thin film is epitaxially grown on a latticemismatched substrate, has found its application in many areas [44]. SLs and QWs are high-quality multilayered structures grown from lattice matched and mismatched materials.

38

PROPERTIES OF SEMICONDUCTOR ALLOYS

The large lattice mismatch is totally accommodated by uniform elastic strains in the layers if the layer thicknesses are kept below certain critical values. The idea for thin films emerged from a critical layer thickness hc below which a dislocation-free, coherently strained interface would be stable and above which a misfit dislocation structure and semi-coherent interface would be stable. Knowledge of the so-called critical thickness is essential for realizing the advantages of lattice-mismatched heterostructure systems. The critical thickness hc of an epilayer, which was first considered by Frank and van der Merwe [45], is a parameter introduced to explain the experimental observation of coherent, pseudomorphic or strained-layer epitaxy. The breakdown of coherency can be determined in several ways. XRD and PL are commonly employed methods of determining the loss of coherency by demonstrating a change in average lattice constant (XRD) or a shift in PL peak energy and a reduction in PL intensity, following the release of strain. TEM is the direct manifestation of the breakdown of coherency. We show in Figure 1.29 the critical thickness hc versus x for (a) SixGe1x layer on Si, (b) GaxIn1xAs layer on InP and (c) GaNxAs1x layer on GaAs, respectively. Note that x ¼ 0.47 in Figure 1.29(b) is the lattice-matching composition to InP. 104

(a) SixGe1-x /Si

102

hc (Å)

100

0

104

0.2

0.4

0.6

0.8

1.0

0.6

0.8

1.0

(b) Gax In1-x As/InP

102 100

0

0.2

0.4

104

(c) GaNx As1-x /GaAs

102 100

0

0.02

0.04

0.06

0.08

0.10

x

Figure 1.29 Critical thickness hc versus x for (a) SixGe1x layer on Si, (b) GaxIn1xAs layer on InP and (c) GaNxAs1x layer on GaAs. The solid lines represent the theoretical model of Matthews and Blakeslee [46]. The heavy solid line in (a) is obtained from an energy-balanced misfit dislocation generation model by People and Bean [47]

Although several theories have been proposed to predict hc [44], most semiconductor device designers rely upon the model of Matthews and Blakeslee [46]. The solid lines in Figure 1.29 show the results based on this model. The experimental hc data usually exceed the Matthews–Blakeslee’s prediction. It is also understood that for SixGe1x there is little dependence of hc on x. The heavy solid line in Figure 1.29(a) represents the theoretical curve obtained from an energy-balanced misfit dislocation generation model by People and Bean [47]. This model is in excellent agreement with the experimental data. The critical thicknesses hc for AlxGa1xN and GaxIn1xN on relaxed GaN layers were measured by Akasaki and Amano [48]. The experimental hc values were in the range 300 to 700 nm for AlxGa1xN/GaN (0.05 x 0.2) and 40 nm for GaxIn1xN/GaN (0.8 x 0.95).

STRUCTURAL PROPERTIES

39

The hc values for SixGe1x/Si and some III–V and II–VI semiconductors grown on various lattice-mismatched substrates are summarized in Figure 1.30. The solid lines are obtained by least-squares fitting with (hc in A, Da/a in at%) A n hc ¼ ð1:25Þ Da=a with A ¼ 7.5 and n ¼ 3.5 for SixGe1x/Si, A ¼ 16 and n ¼ 2.4 for III–V semiconductors and A ¼ 52 and n ¼ 1.5 for II–VI semiconductors. It should be noted that the II–VI semiconductors have weak bond strength. The dislocation energy in such semiconductors is much smaller than those in SixGe1x/Si and III–V semiconductors. Therefore, dislocations can be more easily generated in the II–VI semiconductors. 104

(a) SixGe1-x /Si

102

hc (Å)

100 104 102

(b) III-V semiconductors

100 104 102

(c) II-VI semiconductors 100 -2 10 10-1 100 Δa/a (%)

101

Figure 1.30 Critical thickness hc for (a) SixGe1x, (b) III–V and (c) II–VI semiconductors grown on various lattice-mismatched substrates. The solid lines represent the least-squares fit using Equation (1.25)

1.6 STRUCTURAL PHASE TRANSITION At high pressure the group-IV elemental semiconductors show metallic transitions in a sequence from cubic (diamond) ! tetragonal (b-Sn) ! simple hexagonal ! hexagonal close packed. Similarly, the III–V and II–VI binary semiconductors exhibit a variety of the crystal structures at high pressures. In Tables 1.8 and 1.9 of Adachi [1], transition pressure to the first phase (PT) and transition sequences can be found for some group-IV, III–V and II–VI semiconductors. The additional data are: PT ¼ 56 GPa (zinc-blende ! hexagonal (NiAs)) for BeSe; PT ¼ 35 GPa (zincblende ! hexagonal (NiAs)) for BeTe; and PT ¼ 90.6 GPa (rocksalt ! CsCl) for CdO. There are a very few studies on the structural phase transition in semiconductor alloys. Some of these studies are summarized in Table 1.16. Webb et al. [49] observed the phase transition in ZnxCd1xTe from the zinc-blende to rocksalt structures. However, the recent studies on ZnTe and CdTe suggest the presence of cinnabar phase between the zinc-blende and rocksalt structures [50]. Vnuk et al. [51] studied the effect of pressure on semiconductor

40

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 1.16 Phase-transition sequence observed for some III–V and II–VI ternaries at high pressures. zb ¼ zinc-blende; or ¼ orthorhombic; w ¼ wurtzite; rs ¼ rocksalt (NaCl); cin ¼ cinnabar System

Material

Sequence

Ref.

III–V

GaxIn1xP AlxGa1xAs GaxIn1xSb

semiconductor ! metal (optical absorption) zb ! or (Pmm2)/or (Cmcm) (GaAs like) zb ! b-Sn

a b c

II–VI

MgxZn1xO ZnxCd1xS ZnxCd1xSe

w ! rs zb ! rs zb ! rs (x ¼ 0.9) semiconductor ! metal (0 x 0.32) zb ! rs semiconductor ! metal (resistance) zb ! cin ! rs (0 x 0.55) zb ! rs (0.55<x 1)

d e f g h i j j

ZnxCd1xTe ZnSxSe1x ZnSexTe1x

A. R. Go~ ni et al., Phys. Rev. B 39, 3178 (1989) W. Paszkowicz et al., Acta Phys. Pol. A, 91, 993 (1997) c C. Y. Liu et al., J. Phys. Chem. Solids 39, 113 (1978) d J. A. Sans and A. Segura, High Pressure Res. 24, 119 (2004) e A. Beliveau and C. Carlone, Phys. Rev. B 44, 3650 (1991) f C.-M. Lin et al., Phys. Rev. B 58, 16 (1998) g Y. C. Lin et al., J. Appl. Phys. 101, 073507 (2007) h A. W. Webb et al., J. Appl. Phys. 61, 2492 (1987) i S. R. Tiong et al., Jpn. J. Appl. Phys. 28, 291 (1989) j J. Pellicer-Porres et al., Phys. Rev. B 71, 035210 (2005) a b

(a-Sn)-to-metal (b-Sn) transition temperature in dilute GexSn1x (x 1 at%). They obtained a slope of 48.4 6 K/kbar, in good agreement with thermodynamic prediction. Figure 1.31 plots the transition pressure to the first phase PT versus x for GaxIn1xSb. The experimental data are taken from Liu et al. [52]. A slight bowing can be found in the PT versus

7

PT (GPa)

6 5

β -Sn

4 3

zb

2 Gax In1-x Sb

1 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 1.31 Transition pressure to the first phase PT versus x for GaxIn1xSb. The experimental data are taken from Liu et al. [52]. The solid line shows the quadratic-fit result using Equation (1.26). zb ¼ zinc-blende

STRUCTURAL PROPERTIES

41

x plots. The solid line shows the best-fit result of the quadratic expression (in GPa) PT ðxÞ ¼ 2:3 þ 6:5x2:6x2

ð1:26Þ

PT (GPa)

The transition pressures to the first phase PT against alloy composition x for some II–VI semiconductors are shown in Figure 1.32. The experimental data are taken for ZnxCd1xS from Beliveau and Carlone [53], for ZnSxSe1x from Tiong et al. [54] and for ZnSexTe1x from Pellicer-Porres et al. [55]. In Figure 1.32(c), the transition pressure to the second phase is also plotted with the open circles. The linear interpolation is concluded to be an efficient tool to estimate the phase transition pressure in semiconductor alloys. 20 15 10 5 0 16 15 14 13 12 20

(a) ZnxCd1-xS

zb m

(b) ZnSxSe1-x

s

rs

cin

15 10 5

rs

zb

0

0.2

0.4

(c) ZnSexTe1-x x

0.6

0.8

1.0

Figure 1.32 Transition pressures to the first phase PT against x for (a) ZnxCd1xS, (b) ZnSxSe1x and (c) ZnSexTe1x. The transition pressure to the second phase is plotted in (c) by the open circles. The experimental data are taken for (a) ZnxCd1xS from Beliveau and Carlone [53], for (b) ZnSxSe1x from Tiong et al. [54] and for (c) ZnSexTe1x from Pellicer-Porres et al. [55]. cin ¼ cinnabar; m ¼ metal; rs ¼ rocksalt (NaCl); s ¼ semiconductor; zb ¼ zinc-blende

1.7 CLEAVAGE PLANE 1.7.1 Cleavage The cleavage properties of a crystal are strongly related to the atomic arrangement and corresponding electron density map. The most readily cleaved crystallographic planes can then be determined only by the crystalline structure. They are (111) plane for alloys of diamond type, (1 1 0) plane for zinc-blende type, ð11 20Þ and ð1010Þ planes for wurtzite type and (100) plane for rocksalt type [1].

1.7.2 Surface Energy The cleavage energy is assumed equal to twice the surface energy of that plane. There is a dearth of experimental measurements on surface energy. The surface energies for several group-VI elemental, III–Vand II–VI binary semiconductors are listed in Tables 1.11–1.13 of Adachi [1]. No surface energy data are available for semiconductor alloys.

42

PROPERTIES OF SEMICONDUCTOR ALLOYS

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons Ltd, Chichester, 2005. [2] A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys, Kluwer Academic, New York, 2002. [3] A. Ourmazd and J. C. Bean, Phys. Rev. Lett. 55, 765 (1985). [4] J. Schilz and V. N. Romanenko, J. Mater. Sci.: Mater. Electron. 6, 265 (1995). [5] T. S. Kuan, T. F. Kuech, W. I. Wang, and E. L. Wilkie, Phys. Rev. Lett. 54, 201 (1985). [6] T. Suzuki, in A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys, Kluwer Academic, New York, 2002, p. 1. [7] A. Gomyo, M. Sumino, I. Hino, and T. Suzuki, Jpn. J. Appl. Phys. 34, L469 (1995). [8] A. Gomyo, K. Makita, I. Hino, and T. Suzuki, Phys. Rev. Lett. 72, 673 (1994). [9] A. A. Mbaye, L. G. Ferreira, and A. Zunger, Phys. Rev. Lett. 58, 49 (1987). [10] H. S. Lee, S. Yi, T. W. Kim, Y. J. Park, J. Y. Lee, M. S. Kwon, and H. L. Park, Solid State Commun. 137, 70 (2006). [11] R. A. Soref, Proc. IEEE 81, 1687 (1993). [12] E. T. Croke, A. T. Hunter, C. C. Ahn, T. Laursen, D. Chandrasekhar, A. E. Bair, D. J. Smith, and J. W. Mayer, J. Cryst. Growth 175–176, 486 (1997). [13] P. C. Kelires, Phys. Rev. B 55, 8784 (1997). [14] M. Berti, D. D. Salvador, A. V. Drigo, F. Romanato, J. Stangl, S. Zerlauth, F. Sch€affler, and G. Bauer, Appl. Phys. Lett. 72, 1602 (1998). [15] J. P. Dismukes, L. Ekstrom, and R. J. Paff, J. Phys. Chem. 68, 3021 (1964). [16] M. Matsuura, J. M. Tonnerre, and G. S. Cargill III, Phys. Rev. B 44, 3842 (1991). [17] H. Kajiyama, S. Muramatsu, T. Shimada, and Y. Nishino, Phys. Rev. B 45, 14005 (1992). [18] I. Yonenaga, M. Sakurai, M. H. F. Sluiter, Y. Kawazoe, and S. Muto, J. Mater. Sci.: Mater. Electron. 16, 429 (2005). [19] N. S. Takahashi, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 3. [20] R. E. Nahory, M. A. Pollack, W. D. Johnston, Jr., and R. L. Barns, Appl. Phys. Lett. 33, 659 (1978). [21] F. Germini, C. Bocchi, C. Ferrari, S. Franchi, A. Baraldi, R. Magnanini, D. D. Salvador, M. Berti, and A. V. Drigo, J. Phys. D: Appl. Phys. 32, A12 (1999). [22] J. D. Bearch, H. Al-Thani, S. McCray, R. T. Collins, and J. A. Turner, J. Appl. Phys. 91, 5190 (2002). [23] L. T. Romano, B. S. Krusor, M. D. McCluskey, and D. P. Bour, Appl. Phys. Lett. 73, 1757 (1998). [24] M. E. Aumer, S. F. LeBoeuf, F. G. McIntosh, and S. M. Bedair, Appl. Phys. Lett. 75, 3315 (1999). [25] G. Bisognin, D. D. Salvador, C. Mattevi, M. Berti, A. V. Drigo, G. Ciatto, L. Grenouillet, P. Duvaut, G. Gilet, and H. Mariette, J. Appl. Phys. 95, 48 (2004). [26] S. Z. Wang, S. F. Yoon, W. J. Fan, W. K. Loke, T. K. Ng, and S. Z. Wang, J. Appl. Phys. 96, 2010 (2004). [27] G. Fournet, J. Phys. Radium 14, 374 (1953). [28] J. C. Mikkelsen, Jr., and J. B. Boyce, Phys. Rev. Lett. 49, 1412 (1982); Phys. Rev. B 28, 7130 (1983) [29] H. Oyanagi, Y. Takeda, T. Matsushita, T. Ishiguro, and A. Sasaki, in Gallium Arsenide and Related Compounds, IOP, Bristol, 1986, p. 295. [30] N. J. Jeffe, A. V. Blant, T. S. Cheng, C. T. Foxon, C. Bailey, P. G. Harrison, J. F. W. Mosselmans, and A. J. Dent, Mater. Res. Soc. Symp. Proc. 512, 519 (1998). [31] T. Mattila and A. Zunger, J. Appl. Phys. 85, 160 (1999). [32] M. Schenk, I. H€ahnert, L. T. H. Duong, and H.-H. Niebsch, Cryst. Res. Technol. 31, 665 (1996). [33] E. Cruceanu and D. Niculesciu, Compt. Rend. Acad. Sci. 261, 935 (1965). [34] K. Ohata, J. Saraale, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1198 (1973). [35] D. A. Wood, K. D. Rogers, D. W. Lane, G. J. Conibeer, and D. Parton, J. Mater. Sci. Lett. 17, 1511 (1998).

STRUCTURAL PROPERTIES

43

[36] N. Motta, A. Balzarotti, P. Letardi, A. Kisiel, M. T. Czyzyk, M. Zimnal-Starnawska, and M. Podgorny, Solid State Commun. 53, 509 (1985). [37] I. C. Noyan and A. Segm€uller, J. Appl. Phys. 60, 2980 (1986). [38] K. Oe and K. Sugiyama, Appl. Phys. Lett. 33, 449 (1978). [39] H. Nagai, J. Appl. Phys. 45, 3789 (1974). [40] K. Uesugi, N. Morooka, and I. Suemune, Appl. Phys. Lett. 74, 1254 (1999). [41] T. Sepp€anen, L. Hulman, J. Birch, M. Beckers, and U. Kreissig, J. Appl. Phys. 101, 043519 (2007). [42] A. Ohtomo, M. Kawasaki, T. Koida, K. Masubuchi, H. Koinuma, Y. Sakurai, Y. Yoshida, T. Yasuda, and Y. Segawa, Appl. Phys. Lett. 72, 2466 (1998). [43] A. B. M. A. Ashrafi and Y. Segawa, J. Vac. Sci. Technol. B 23, 2030 (2005). [44] S. Jain, M. Willander, and R. Van Overstraeten, Compound Semiconductors Straiend Layers and Devices. Kluwer Academic. Boston, 2000. [45] F. C. Frank and J. H. van der Merwe, Proc. Roy. Soc. A 201, 261 (1950). [46] J. W. Matthews and A. E. Blakeslee, J. Cryst. Growth 27, 118 (1974). [47] R. People and J. C. Bean, Appl. Phys. Lett. 49, 229 (1986). [48] I. Akasaki and H. Amano, in Semiconductors and Semimetals, Vol. 50 (edited by J. I. Pankove and T. D. Moustakas), Academic, New York, 1998, p. 459. [49] A. W. Webb, S. B. Qadri, E. R. Carpenter, Jr., E. F. Skelton, and J. Kennedy, J. Appl. Phys. 61, 2492 (1987). [50] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Semiconductors. Kluwer Academic, Boston, 2004. [51] F. Vnuk, A. D. Monte, and R. W. Smith, J. Appl. Phys. 55, 4171 (1984). [52] C. Y. Liu, I. L. Spain, and E. F. Skelton, J. Phys. Chem. Solids 39, 113 (1978). [53] A. Beliveau and C. Carlone, Phys. Rev. B 44, 3650 (1991). [54] S. R. Tiong, M. Hiramatsu, Y. Matsushima, and E. Ito, Jpn. J. Appl. Phys. 28, 291 (1989). [55] J. Pellicer-Porres, D. Martınez-Garcıa, Ch. Ferrer-Roca, A. Segura, and V. Mu~ noz-Sanjose, Phys. Rev. B 71, 035210 (2005).

2 Thermal Properties 2.1 MELTING POINT AND RELATED PARAMETERS 2.1.1 Phase Diagram (a) Group-IV semiconductor alloy Figure 2.1 shows the phase diagram for the Si–Ge system at temperatures near the melting point. The experimental data are taken from various sources. The solid lines show the quadratic fit results (in C) Solidus surface :

Ts ðxÞ ¼ 937 þ 244x þ 231x2

ð2:1aÞ

Liquidus surface :

Tl ðxÞ ¼ 937 þ 916x442x2

ð2:1bÞ

The phase diagram in Figure 2.1 suggests that Si and Ge are completely miscible as liquid and as solid. Stable phases formed by Si and Ge are the liquid and a cubic diamond-type substitutional solid solution. No phase changes or decompositions were detected roentgenographically after annealing homogeneous SixGe1x solid solutions for several months at temperatures in the range 177–925 C [1]. At high pressures above 15 GPa, the bct structure of a Si–Ge solid solution is estimated to be more stable than the diamond structure [2]. The Si–Ge system is a typical representative of a system with strong segregation, i.e. a solid solution in which the solid and liquid phases are separated by a large regime of coexistence. (b) III–V semiconductor alloy A series of papers demonstrated the feasibility of calculating phase diagrams in III–V ternary systems based upon the regular or quasichemical equilibrium model for the solid and liquid phases [3–5]. Because of the small lattice difference between GaAs and AlAs, their solid solutions are the closest in the III–V semiconductor systems to being ideal and the alloys are among the easiest to prepare by LPE. A perspective diagram depicting the solidus surface, liquidus surface and binary boundaries of the Al–Ga–As ternary system is shown in Figure 2.2(a). Figure 2.2(b) also shows the pseudobinary phase diagram of AlAs–GaAs system. We can see in Figure 2.2 that AlAs and GaAs are completely miscible as liquid and as solid. Stable phases formed by these binary compounds are the liquid and a cubic zinc-blende substitutional solid solution of Al and Ga atoms in the cation site. The solid lines in Figure 2.2(b) represent the solidus and liquidus surfaces (in C) [6] Solidus surface : Liquidus surface :

Ts ðxÞ ¼ 123854x þ 560x2

ð2:2aÞ

Tl ðxÞ ¼ 1238 þ 1082x580x2

ð2:2bÞ

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

46

PROPERTIES OF SEMICONDUCTOR ALLOYS 1500 1400

SixGe1-x

1300 T (°C)

Liquid 1200 1100

Solid + Liquid

1000 Solid

900 800

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.1 Normal-pressure phase diagram of a Si–Ge system. The solid lines represent the quadratic fits using Equation (2.1)

Figure 2.2 (a) Perspective diagram depicting the solidus surface, liquidus surface and binary boundaries in the Al–Ga–As ternary system. (b) Solidus and liquidus curves for the AlAs–GaAs pseudobinary system. The solid lines in (b) represent the solidus and liquidus surfaces calculated from Equation (2.2)

Figure 2.3 shows the solidus and liquidus curves for (a) GaP–InP, (b) GaAs–InAs and (c) GaSb–InSb systems. These systems provided a homogeneous series of alloys differing only in the anion substitution. The pseudobinary GaSb–InSb system can be approximated by the quadratic expressions (in C) Solidus surface :

Ts ðxÞ ¼ 52472x þ 261x2

ð2:3aÞ

Liquidus surface :

Tl ðxÞ ¼ 524 þ 280x90x2

ð2:3bÞ

This is not the case for the GaP–InP and GaAs–InAs systems, as seen in Figures 2.3(a) and 2.3(b).

THERMAL PROPERTIES

47

1600 (b) GaxIn1-xAs

Liquid

(c) GaxIn1-xSb

1400 Liquid

T (°C)

1200 1000 Solid

Solid

800

Liquid

600 (a) GaxIn1-xP

Solid

400 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x

Figure 2.3 Solidus and liquidus curves for (a) GaP–InP, (b) GaAs–InAs and (c) GaSb–InSb pseudobinary systems. The solid lines in (c) represent the solidus and liquidus surfaces calculated from Equation (2.3)

GaxIn1xN is a random alloy having the wurtzite structure. Due to the large difference (11%) in the lattice constants between GaN and InN, the solid solution has a tendency to undergo phase separation. It is possible to grow thin epitaxial GaxIn1xN layers with the cubic structure. The phase stability of GaxIn1xN has been the subject of several experimental [7,8] and theoretical studies [9–15]. We reproduce in Figure 2.4 the pseudobinary diagram of zinc-blende and wurtzite GaxIn1xN obtained theoretically by Gan et al. [15]. A direct comparison of the predicted phase diagram to an experimental phase diagram cannot be made since the latter has never been determined. However, an experimental study on Ga0.91In0.09N [8] suggested that this alloy does 1800 Zinc-blende

T (K)

1600

1400

Wurtzite

1200

GaxIn1-xN

1000 0

0.2

0.4

x

0.6

0.8

1.0

Figure 2.4 Pseudobinary phase diagram of zinc-blende and wurtzite GaxIn1xN. The solid and open circles represent the experimental data for which phase separation was and was not observed, respectively; data taken from Doppalapudi et al. [8]. [Reprinted with kind permission from C. K. Gan, Y. P. Feng, and D. J. Srolovitz, Phys. Rev. B 73, 235214 (2006). Copyright (2006) by the American Physical Society]

48

PROPERTIES OF SEMICONDUCTOR ALLOYS

not phase separate at the growth temperature of 923 K. The corresponding data point (x, T) ¼ (0.09, 923 K) is shown by the open circle in Figure 2.4. It lies in the region between the binodal and spinodal, suggesting that the solid solution is metastable with respect to phase segregation. Additional experimental points in Figure 2.4 show that phase separation occurs in both Ga0.63In0.37N and Ga0.65In0.35N grown at 998 K (solid circles) [8], in agreement with the predicted phase diagram (i.e. the data fall in the spinodal region). Gan et al. [15] suggested that the wurtzite structure is thermodynamically more stable than the zinc-blende structure at all temperatures and alloy compositions. They also demonstrated that the lattice vibrations can drastically alter the thermodynamic properties and phase diagram of GaxIn1xN. (c) II–VI semiconductor alloy Figure 2.5 shows the phase diagram of the MgO–ZnO system at 4.4 GPa (solid lines) and at ambient pressure (dashed lines). The ambient and high-pressure diagrams are taken from Raghavan et al. [16] and Solozhenko et al. [17], respectively. At ambient pressure [16], the MgO–ZnO system is of eutectic type and is characterized by the extensive solubility of ZnO in MgO and the restricted solubility of MgO in ZnO. The two-phase region in the MgO–ZnO system extends from 3.5 to 70.5 mol% ZnO at 1000 C and becomes narrower at higher temperatures. Solozhenko et al. [17] observed a phase transition of w-MgxZn1xO solid solution into rocksalt by stepwise heating at various temperatures. The quenching of the 4000 Mgx Zn1-xO L 3400 L+rs-MZO

T (ºC)

2800

2200 rs-MZO

rs-MZO + w-MZO

1600

w-MZO 1000 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.5 Phase diagram of MgO–ZnO pseudobinary system at ambient pressure taken from Raghavan et al. [16] (dashed lines) and at 4.4 GPa (solid lines). MZO ¼ MgZnO; L ¼ liquid; rs ¼ rocksalt; w ¼ wurtzite. [Reprinted with permission from V. L. Solozhenko et al., Solid State Commun. 138, 534–537 (2006), Copyright (2006) Elsevier]

THERMAL PROPERTIES

49

reaction mixtures resulted in the formation of stable MgxZn1xO solid solutions with the rocksalt structure. The phase diagram at 4.4 GPa in Figure 2.5 was proposed based on these facts [17]. Figure 2.6 shows the ZnTe–CdTe solidus and liquidus curves. The experimental data are taken from Steininger et al. [18]. XRD measurements indicated that ZnxCd1xTe forms a complete series of solid solutions with lattice parameters varying almost linearly with x. The solidus and liquidus curves in Figure 2.6 represent monotonic and sublinear variations with x from the melting point of CdTe to that of ZnTe. This type of x versus T variation suggests small and nearly comparable positive deviations from ideality in the solid and liquid phases and is similar to those observed in other II–VI systems, such as ZnSe–ZnTe [19], CdSe–CdTe [20] and HgSe–HgTe (Figure 2.9).

T (°C)

1300

ZnxCd1-xTe

Liquid

1200

Solid 1100 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.6 Solidus and liquidus curves for ZnTe–CdTe pseudobinary system. The experimental data are taken from Steininger et al. [18]. The solid lines represent the solidus and liquidus surfaces calculated from Equation (2.4)

The solid lines in Figure 2.6 represent the quadratic expressions (in C) Solidus surface : Ts ðxÞ ¼ 1092 þ 30x þ 173x2 Liquidus surface : Tl ðxÞ ¼ 1092 þ 131x þ 72x2

ð2:4aÞ ð2:4bÞ

Of particular interest in Figure 2.6 is the slow increase in liquid temperatures and the relatively narrow gap between solidus and liquidus curves (less than 0.16 mole fraction). These are very favorable for the growth of alloys from the melts in standard quartz ampoules up to relatively high values of Zn content [21]. The CdS–CdTe system has different crystal structures, that is, the zinc-blende and wurtzite structures, when prepared high temperatures. Early studies on this alloy system failed to produce mixed crystals for the full range of compositions, concluding that a large miscibility gap exists in the CdS–CdTe system. More recently, Ohata et al. [22] studied the system for the full range of compositions and observed a change of phase from the zinc-blende to wurtzite at x 0.2. Wood et al. [23] confirmed using PIXE and XRD that bulk CdSxTe1x alloy has the zinc-blende structure for x 0.2 and the wurtzite structure for x 0.25. Figure 2.7 shows the phase diagram of the CdS–CdTe system obtained by these authors [22,23]. Figure 2.8 illustrates the phase diagram for the CdSe–CdTe system [21]. This system and the ZnTe–CdTe system in Figure 2.6 show typical ‘lens-shape’ phase diagrams with sublinear

50

PROPERTIES OF SEMICONDUCTOR ALLOYS

CdSxTe1-x

1400

Liquid

Liquid+ Solid

T (ºC)

1200

1000 Wurtzite 800

Zinc-blende+ Wurtzite

Zinc-blende 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.7 Phase diagram of CdS–CdTe pseudobinary system. The experimental curves are taken from Ohata et al. [22] and Wood et al. [23]

variations in temperature with composition and relatively narrow solidus–liquidus gaps. The CdSe–CdTe system represents almost the same type of solidus–liquidus diagram with a degenerate eutectic near 20 mol% CdSe. The narrow zincblende–wurtzite two-phase region inside the solidus field shows increasing stability of the wurtzite phase with increasing temperature.

Figure 2.8 Phase diagram of CdSe–CdTe pseudobinary system. [Reprinted with permission from J. Cryst. Growth, Phase diagrams and crystal growth of pseudobinary alloy semiconductors by J. Steininger and A. J. Strauss, 13–14, 657. Copyright (1972), Elsevier]

THERMAL PROPERTIES

51

800 HgSexTe1-x 750 T (°C)

Liquid

700

Solid

650 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.9 Phase diagram of HgSe–HgTe pseudobinary system. The experimental data are taken from Harman [24]. The solid lines represent the solidus and liquidus surfaces calculated from Equation (2.5)

Harman and Strauss [24] determined the phase diagram for the HgSe–HgTe system. The liquidus data in Figure 2.9 were measured by differential thermal analysis of cooling curves, while the solidus points were obtained by determining the composition of the alloys that were the first to freeze from melts of known composition [24]. The solidus and liquidus curves show a very small separation (about 3 mol% between 25 and 75 mol% HgSe). The solid lines in Figure 2.9 represent the quadratic expressions (in C) Solidus surface : Liquidus surface :

Ts ðxÞ ¼ 67012x þ 141x2

ð2:5aÞ

2

ð2:5bÞ

Tl ðxÞ ¼ 670 þ 3x þ 127x

2.1.2 Melting Point The melting point Tm is one of the most essential thermophysical parameters. Some thermophysical parameters, including Tm, for a number of group-IV, III–Vand II–VI semiconductors are summarized in Table 2.1. Figure 2.10 shows the melting point Tm versus x for CxSi1x. The open circles show the experimental data for diamond and Si, while the solid circle represents the 3C-SiC (x ¼ 0.5) data. The solid line represents Vegard law. It predicts generally acceptable alloy values. We have, however, already shown in Section 2.1.1 that a quadratic function or a higher-order polynomial can be fitted to the solidus curves of many alloys. Therefore, attention should be paid to the estimation of Tm using the linear interpolation scheme.

2.2 SPECIFIC HEAT 2.2.1 Group-IV Semiconductor Alloy Specific heat is a strongly temperature-dependent quantity [25]. There has been no experimental data on the specific heat of group-IV semiconductor alloys. Kagaya et al. [26]

52

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 2.1 Melting point Tm, specific heat Cp, Debye temperature uD, thermal expansion coefficient ath and thermal conductivity K for some group-IV, III–V and II–VI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)); rs ¼ rocksalt; rh ¼ rhombohedral System

Material

Tm (K)

Cp (J/g K)

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb) 2H-SiC (w)

4100a 1687 1210.4

0.5148 0.713 0.3295b 0.278c 0.677e

1870 643 348b 238c 1122

III–V

II–VI

2810 2810

uD (K)

BN (zb) BN (h)

> 3246 > 3246

0.643 0.805

1613 323

BP (zb) BAs (zb) AlN (zb) AlN (w)

> 3300 2300 3487 3487

0.75 0.408

1025i 800

0.728

988

AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaN (w)

2823 2013 1338 2791 2791

0.727 0.424 0.326b

687 450 370b

0.42

821

GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InN (w)

1730 1513 991 2146 2146

0.313 0.327 0.344b

493k 370 240b

2.274

674

InP (zb) InAs (zb) InSb (zb)

1335 1210 797

0.322 0.352 0.350b

420b 280b 161b

BeO (w)

2851

1.029

1280

0.83

900

3250 2783o 1560 > 1300 1975 1975

0.928

745

0.497

416

2196

0.486

440

BeS (zb) BeTe (zb) MgO (rs) MgS (rs) MgSe (zb) MgTe (w) ZnO (zb) ZnO (w) ZnS (zb)

ath (106 K1) 1.05 2.616 5.75 5.25d 2.77 1.15 2.75 (?c) 38.0 (jjc) 2.94 3.042 (?c) 2.227 (jjc) 4.28 4.2j 5.0 (?c) 4.5 (jjc) 4.89 6.03 6.35 3.830 (?c) 2.751 (jjc) 4.56 5.50m 5.04 7.2 (?c)n 6.0 (jjc)n 7.66 10.5

4.31 (?c) 2.49 (jjc) 6.71

K (W/cm K) 22 1.56 0.6 3.4f 13g 3.9h 3.5 3.19h 0.9 0.91 0.57 1.95h 0.77 0.45 0.36 0.45h,l 0.68 0.3 0.165–0.185 3.7h

0.52

0.54h 0.27 (continued)

THERMAL PROPERTIES

53

Table 2.1 (Continued ) System

Material

Tm (K)

ZnS (w)

2196

ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdS (w)

1793 1568 1700 1748 1748

CdSe (zb) CdSe (w)

1531 1531

CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

1365 1723 1072 943

Cp (J/g K)

uD (K) 351

ath (106 K1)

K (W/cm K)

6.54 (?c) 4.59 (jjc) 7.8 8.33 14

0.17h,p

0.20h,q

0.360 0.258 0.340

340 260 255

0.3280

310

4.30 (?c) 2.77 (jjc)

0.281

135

0.211

185

0.355 0.162

242 143

4.13 (?c) 2.76 (jjc) 4.70 4.3r 1.41 4.70

0.19 0.18 0.007

0.09h 0.075 0.001–0.035 0.0238

At 12.5 GPa At 273 K c At 100 K d At 220 K e Cv value f At 290 K g Estimated h This semiconductor has two tensor components, K? and Kjj; however, the difference between K? and Kjj appears to be less than the experimental uncertainty at room temperature i At 320 K j At 280 K k At 150 K l Ceramics m Obtained from an analysis of GaInPAs quaternary data n At 373 K o Theoretical p Note that the w-ZnS crystal used in the experiment may be faulted; therefore, the value for this crystal is much smaller than that for c-ZnS q At 283 K r T ¼ 484 621 K a b

investigated theoretically the specific heat of SixGe1x from 0 to 500 K. The difference in specific heat between at constant pressure and constant volume Cp–Cv was found to be negligible at low temperatures, but increased by less than 3–3.5% at 500 K. The calculated Cp values fell between the endpoint values of Si and Ge. Figure 2.11 shows the specific heat Cp versus x for CxSi1x at 300 K. The experimental data for diamond, Si and 3C-SiC (x ¼ 0.5) are shown by the open and solid circles. The dashed line represents the linear interpolation result between the experimental diamond and Si values written as (in J/g K) Cp ðxÞ ¼ 0:7130:198x

ð2:6Þ

54

PROPERTIES OF SEMICONDUCTOR ALLOYS 5000 4000

CxSi1-x

Tm (K)

3000 2000 3C-SiC 1000 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.10 Melting point Tm versus x for CxSi1x. The open and solid circles show the experimental data. The solid line represents the result of Vegard law between diamond and Si 1.0

Cp (J/g K)

0.8 0.6 0.4

3C-SiC

0.2

Cx Si 1-x

0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.11 Specific heat Cp versus x for CxSi1x at 300 K. The open and solid circles show the experimental data. The dashed line shows the linear interpolation result given by Equation (2.6), while the solid line is calculated from Equation (2.7)

The linear interpolation is concluded to estimate generally acceptable alloy Cp values. The solid line in Figure 2.11 shows the result of quadratic fit (in J/g K) Cp ðxÞ ¼ 0:713 þ 0:051x0:245x2

ð2:7Þ

2.2.2 III–V Semiconductor Alloy Sirota et al. [27] determined the Cp and Cv values of InPxAs1x from 5 to 160 K and their Cp data obtained at 160 K are shown graphically in Figure 2.12. The solid line shows the linear interpolation result between InP and InAs (in J/g K) Cp ðxÞ ¼ 0:220 þ 0:027x The linear interpolation scheme is found to yield generally acceptable alloy values.

ð2:8Þ

THERMAL PROPERTIES

55

0.26 In Px As 1-x Cp (J/g K)

0.24

0.22 T=160 K 0.20

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.12 Specific heat Cp versus x for InPxAs1x at 160 K. The experimental data are taken from Sirota et al. [27]. The solid line shows the linear interpolation result between the endpoint binary data

Sirota et al. [28] measured the Cp and Cv values of (GaAs)x(InP)1x quaternary from 5 to 300 K. Figure 2.13 shows the Cp data measured at 300 K. The solid line represents the result of linear interpolation given by (in J/g K) Cp ðxÞ ¼ 0:309 þ 0:014x

ð2:9Þ

0.34

Cp (J/g K)

0.32

0.30 (GaAs)x(InP)1-x 0.28

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.13 Specific heat Cp versus GaAs composition x for (GaAs)x(InP)1x at 300 K. The experimental data are taken from Sirota et al. [28]. The solid line shows the linear interpolation result between the endpoint binary data

It should be noted that the GaAs and InP values of 0.323 and 0.309 J/g K reported by Sirota et al. [28] are slightly smaller than those listed in Table 2.1. It can be seen in Figure 2.13, however, that the linear interpolation scheme is a useful tool for estimating alloy Cp values. Using the linear interpolation scheme, we obtain Cp versus x (0 x 1.0) and T (300 T 1500 K) for AlxGa1xAs as (Cp in J/g K) [29] Cp ðx; TÞ ¼ ð0:343 þ 0:133xÞ þ ð4:7 þ 1:5xÞ 105 Tð3:2 þ 3:3xÞ 103 T 2

ð2:10Þ

56

PROPERTIES OF SEMICONDUCTOR ALLOYS

2.2.3 II–VI Semiconductor Alloy The specific heat of CdxHg1xTe was measured from 5 to 300 K by Sirota et al. [30] and from room temperature up to 523 K by Gambino et al. [31]. The data of Gambino et al. revealed a remarkable anomaly in the form of an abrupt increase below a ‘step temperature’ which depended on x, as shown in Figure 2.14(a). The step temperature reached a maximum at about mid-range composition. It clearly signified an equilibrium solid-state phase change, which they suggested, could be a miscibility gap. As plotted in Figure 2.14(b), this phase change reaches 358 K at x ¼ 0.253 and might reach 240 K at x ¼ 0.2. Maleki and Holland [32] subjected Gambino’s data to a polynomial fit and summarized their results in tabular form. Sirota et al. [30] mentioned ‘an anomaly’ which caused their data to scatter from 15 to 80 K, but did not observe the phase boundary reported by Gambino et al., possibly because their temperatures were too low [32]. 0.23 x=1.0

0.21

x=0.8

440

(b)

400

Miscibility gap

360 0.20

0

x=0.6

0.19 0.18 0.17

x=0.5 x= 0.253 x=0

Cp (J/g K)

Cp (J/g K)

T (K)

0.22

480 CdxHg1-xTe

(a) 0.16 300 350 400 450 500 550 T(°C)

0.2 0.4 0.6 0.8 1.0 x

0.22 (c) 0.20 0.18 0.16 0

T=500 K

0.2 0.4 0.6 0.8 1.0 x

Figure 2.14 (a) Specific heat Cp versus temperature T for CdxHg1xTe with x ¼ 0 1.0. (b) Miscibility gap versus x for CdxHg1xTe. (c) Specific heat Cp versus x for CdxHg1xTe at 500 K. The experimental data in (a)–(c) were obtained from Gambino et al. [31]. The solid line in (c) shows the linear interpolation result between the endpoint binary data

The Cp versus x data for CdxHg1xTe measured at 500 K by Gambino et al. [31] are shown in Figure 2.14(c). The solid line represents the linear interpolation between CdTe and HgTe. It is understood that Cp can be successfully estimated from the linear interpolation scheme; however, a shallow dip in the experimental Cp–x plots is observed in the region centered at x 0.5. Gambino et al. [31] considered that the dip in Cp at x 0.5 is due to the presence of two phases and to the thermal effect associated with the change in equilibrium (solid $ solid(1) þ solid(2)) during Cp measurement, i.e. sample heating.

2.3 DEBYE TEMPERATURE 2.3.1 General Considerations Principally, the X-ray Debye temperature uD for pure metal can be given by [33] mu2D ¼

9f h2 CkB2 a

ð2:11Þ

THERMAL PROPERTIES

57

where m is the displacement of an atom from its lattice site, f is an average nearest-neighbor force constant, C is a numeric constant which depends on the lattice structure, kB is Boltzmann’s constant and a is the atomic mass unit. For a random alloy, the Debye temperature can be simply written as [33] mu2D ¼

X

xi mi u2Di þ

i

1X Aij xi xj ðmi u2Di þ mj u2Dj Þ 2 i„j

ð2:12Þ

where Aij is the factor accounting for the effect of an alloy disorder on the nearest-neighbor force constant. Although Equation (2.12) is for X-ray Debye temperature, it can also be applied to specificheat Debye temperatures since the two differ by a factor depending on Poisson’s ratio, which does not vary significantly from metal to metal and also from semiconductor to semiconductor [25]. If mi is not dependent on material and Aij is negligibly small, Equation (2.12) can then be simply written as u2D ðxÞ ¼

X

xi u2Di

ð2:13Þ

xi uDi

ð2:14Þ

i

The simplest Vegard law can be expressed as uD ðxÞ ¼

X i

2.3.2 Group-IV Semiconductor Alloy Figure 2.15 shows the Debye temperature uD versus x for CxSi1x at 300 K. The open and solid circles represent the experimental data for diamond, Si and 3C-SiC (x ¼ 0.5). The light solid line is calculated from Equation (2.13), while the dashed line is obtained from Equation (2.14).

2000 Cx Si 1- x

θ D (K)

1500

1000 3C-SiC

500

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.15 Debye temperature uD versus x for CxSi1x at 300 K. The heavy solid, light solid and dashed lines are calculated from Equations (2.12), (2.13) and (2.14), respectively

58

PROPERTIES OF SEMICONDUCTOR ALLOYS

The heavy solid line can also be obtained from Equation (2.12) with m ¼ mi(¼mj) ¼ 1 and Aij ¼ 1.4 (all these quantities are assumed to be non-dimensional). The high Debye temperature reflects low atomic mass and therefore short interatomic bond length in ANB8N semiconductors [25].

2.3.3 III–V Semiconductor Alloy The specific-heat Debye temperature uD for (a) InPxAs1x at 160 K and (b) (GaAs)x(InP)1x at 300 K is shown in Figure 2.16. The experimental data are taken from Sirota et al. [27,28]. The solid lines show the calculated results obtained using Equation (2.14). It was found that the uD versus x data can be satisfactorily explained by this expression. The Debye temperatures for these alloys are also found to vary with temperature in the same way as for the endpoint binaries, passing through a deep minimum in the region 10–20 K [27,28]. 450

θ D (K)

400

T=160 K

350 (a) InPx As1-x

300 250 600

θ D (K)

500

T=300 K

400 300 200

(b) (GaAs)x (InP) 1-x 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.16 Debye temperature uD versus x for (a) InPxAs1x at 160 K and (b) (GaAs)x(InP)1x at 300 K. The experimental data for InPxAs1x are taken from Sirota et al. [27] and for (GaAs)x(InP)1x from Sirota et al. [28]. The solid lines show the results calculated using Equation (2.14)

2.3.4 II–VI Semiconductor Alloy Nikiforov and Sredin [34] determined the specific-heat Debye temperature uD for CdxHg1xTe using a calorimeter. These results are shown in Figure 2.17. The solid line represents the linear interpolation result between the endpoint data in Table 2.1. As in the case of the III–V semiconductor alloys, the Debye temperature of CdxHg1xTe is a smooth and monotonic function of x; however, we can see an abrupt change at x ¼ 0.2. This may be due to an experimental error or may be the effect of any difference in crystalline quality. Since the Debye temperature is a model parameter that cannot be measured directly, it may contain considerable uncertainty, including numeric error.

THERMAL PROPERTIES

59

190 Cd x Hg1-xTe

θ D (K)

180 170 160 150 140 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.17 Debye temperature uD versus x for CdxHg1xTe at 300 K. The experimental data are taken from Nikiforov and Sredin [34]. The solid line shows the linear interpolation result using Equation (2.14) between the endpoint binary data

2.4 THERMAL EXPANSION COEFFICIENT 2.4.1 Group-IV Semiconductor Alloy During cooling down in epitaxial growth, a difference in thermal expansion can produce the driving force that moves the defects in the semiconductor heterostructure. Knowledge of the thermal expansion coefficient is, thus, essential not only from a physical point of view, but also for semiconductor device engineering. Figure 2.18 shows the linear thermal expansion coefficient ath for CxSi1x at 300 K. The experimental data are shown by the open and solid circles. The dashed line represents the 6 CxSi1-x 3C-SiC

4

-6

-1

α th (10 K )

5

3 2 1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.18 Linear thermal expansion coefficient ath versus x for CxSi1x at 300 K. The dashed line represents the linearly interpolated result of Equation (2.15). The solid line shows the quadratic fit of Equation (2.16)

60

PROPERTIES OF SEMICONDUCTOR ALLOYS

linear interpolation between diamond and Si (in 106 K1) ath ðxÞ ¼ 2:621:57x

ð2:15Þ

3C-SiC can be regarded as an alloy of C and Si (x ¼ 0.5); however, the linearly interpolated x ¼ 0.5 value in Figure 2.18 does not show good agreement with the experimental 3C-SiC data. It should be noted that C and Si crystallize in the diamond structure, but 3C-SiC crystallizes in the zinc-blende structure. The solid line in Figure 2.18 represents the quadratic fit (in 106 K1) ath ðxÞ ¼ 2:62 þ 2:03x3:60x2

ð2:16Þ

The ath value for SixGe1x was measured by Zhdanova et al. [35] and their results obtained at temperatures between 473 and 773 K are reproduced in Figure 2.19. The expansion decreased monotonically from Ge to Si. A gradual increase in ath was also found with increasing temperature from 300 K up to 1100 K. In Figure 2.19, there is a sudden change in the slope at x 0.15, which coincides with the transition of electronic properties from Ge-like to Si-like (Figure 6.8).

Figure 2.19 Linear thermal expansion coefficient ath versus x for SixGe1x at 473 and 773 K. [Reprinted from Izv. Akad. Nauk. SSSR Neorg. Mater. 3, 1263 (1967)]

The linear expansion coefficient ath is proportional to the specific heat Cv (Gr€uneisen rule) [25] 1 qa gCv Co ath ¼ ¼ a qT p 3V

ð2:17Þ

THERMAL PROPERTIES

61

where g is the averaged Gr€ uneisen parameter, Cv is the specific heat at constant volume, Co is the isothermal compressibility and V is the volume of the crystal. Theoretical work on ath, g and Cv was carried out by Kagaya et al. [26]. A simplified model was used where the lattice vibrations of Si and Ge atoms in the Si–Ge solid solution were assumed to be those of pure Si and Ge except that the lattice constant of the alloy was used. As in pure Si and Ge, the negative thermal expansion was predicted at low temperatures in SixGe1x.

2.4.2 III–V Semiconductor Alloy Figure 2.20 shows the x dependence of ath for AlxGa1xAs at 300 K. The experimental data are taken from Takahashi [36] and Bak-Misiuk [37]. The result of linear interpolation between AlAs and GaAs is shown by the solid line. The difference in ath between the GaAs substrate and the AlxGa1xAs epilayer can be approximated in Figure 2.20 by (in K1) Dath ðxÞ ¼ 1:75x 106

ð2:18Þ

8 AlxGa1-xAs

6

α th (10

-6

-1

K )

7

5 4 3

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.20 Linear thermal expansion coefficient ath versus x for AlxGa1xAs at 300 K. The experimental data are taken from Takahashi [36] and Bak-Misiuk et al. [37] (open circles). The linear interpolation result between the AlAs and GaAs values is shown by the solid line

The linear thermal expansion coefficients ath plotted against x for GaxIn1xP and GaPxAs1x at 300 K are shown in Figures 2.21(a) and 2.21(b), respectively. The experimental data are taken for GaxIn1xP from Kudman and Paff [38] and Leszczynski et al. [39] and for GaPxAs1x from Straumanis et al. [40]. It is apparent from Figure 2.21(a) that the thermal expansion of GaxIn1xP by Kudman and Paff [38] can be expressed as a linear function of x (solid circles). However, the endpoint values extrapolated from these data seem to be considerably larger than the generally accepted values (Table 2.1). Leszczynski et al. [39] measured the ath value of relaxed Ga0.5In0.5P layers grown on GaAs by LPE and reported it as 4.6 106 K1. This value (open circle) agrees well with the linear interpolation scheme (solid line). The data in Figure 2.21(b) can be approximated by the linear interpolation scheme (solid line). The experimental data can be read more exactly from the dashed curve written as (in 106 K1) ath ðxÞ ¼ 6:033:14x þ 2:00x2

ð2:19Þ

PROPERTIES OF SEMICONDUCTOR ALLOYS 7

7

6

6

5

5

α th (10-6 K-1)

α th (10-6 K-1)

62

4 GaxIn1-xP

3

4

2

2

1 0

GaPxAs1-x

3

1

(a) 0

0.2

0.4

0.6

0.8

0

1.0

(b) 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 2.21 Linear thermal expansion coefficients ath as a function of x for (a) GaxIn1xP and (b) GaPxAs1x at 300 K. The experimental data in (a) are taken from Kudman and Paff [38] (solid circles) and Leszczynski et al. [39] (open circle) and in (b) from Straumanis et al. [40] (open squares). The solid lines in (a) and (b) show the linear interpolation results between the endpoint binary data. The dashed line in (b) represents the result calculated using Equation (2.19)

The x dependence of ath for GaxIn1xPyAs1y has been investigated by many authors (see Adachi [41]). The experimental ath versus y for GaxIn1xPyAs1y/InP at 300 K is plotted in Figure 2.22 [41]. The ath values are found to almost linearly decrease with increasing y. The endpoint binary data are available for GaP, GaAs and InP, but not for InAs (Table 2.1). The solid line in Figure 2.22 represents the linear interpolation expression (in 106 K1) ath ðxÞ ¼ 4:89xy þ 6:03xð1yÞ þ 4:56ð1xÞy þ 5:50ð1xÞð1yÞ

ð2:20Þ

6.0 5.8

GaxIn1-xPyAs1-y / InP

-1

5.4

-6

α th (10 K )

5.6

5.2 5.0 4.8 4.6 4.4 0

0.2

0.4

0.6

0.8

1.0

y

Figure 2.22 Linear thermal expansion coefficients ath versus y for GaxIn1xPyAs1y/InP at 300 K. The experimental data are taken from Adachi [41]. The solid line represents the linear interpolation result of Equation (2.20)

THERMAL PROPERTIES

63

In obtaining Equation (2.20), we assumed the InAs value to be ath ¼ 5.50 106 K1. The linear interpolation expression in Figure 2.22 explains the experimental data satisfactorily. The ath value for AlxGa1xP has also been reported by Bessolov et al. [42].

2.4.3 II–VI Semiconductor Alloy The ath variations in ZnxHg1xTe and CdxHg1xTe have been measured from 4 to 290 K [43]. The bulk crystals were grown by the THM. The negative thermal expansions at temperatures below 65 K were clearly observed in ZnTe, CdTe and HgTe binaries and also in their alloys. The solid circles and triangles in Figure 2.23 show the experimental data measured at 280 K [43]. They are largely scattered. This is especially true for ZnxHg1xTe. 10

α th (10-6 K-1)

9 ZnxHg1-xTe

8 7 6

CdxHg1-xTe

5 4 3

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.23 Linear thermal expansion coefficients ath as a function of x for ZnxHg1xTe and CdxHg1xTe at 280 K. The experimental data are taken from Bagot et al. [43]. The solid lines represent the linear interpolation results between the endpoint binary data

The thermal expansion behaviors were also studied for ZnS0.03Se0.97 from 300 to 550 K [44] and for MgxZn1xSe (0.1 x 0.5) from 10 to 300 K [45]. The negative thermal expansion in conjunction with abnormal temperature dependence of the E0 edge was observed at T 75 K for MgxZn1xSe [45].

2.5 THERMAL CONDUCTIVITY AND DIFFUSIVITY 2.5.1 Thermal Conductivity (a) General considerations An exact calculation of the lattice thermal conductivity K is possible in principle, but lack of knowledge of various material parameters and the difficulty of obtaining an exact solution of phonon– phonon interactions are formidable barriers. In the case of semiconductor alloys, an additional contribution, which is the result of a random distribution of constituent atoms in sublattice sites, should be taken into consideration. A phenomenological model of the lattice thermal conductivity for semiconductor alloys was first proposed by Abeles [46]. His model 2 starts from three kinds of relaxation times: t 1 N ¼ B1 v (three-phonon normal process), 1 2 1 t U ¼ B2 v (three-phonon Umklapp process) and t D ¼ AGv2 (strain and mass point defects),

64

PROPERTIES OF SEMICONDUCTOR ALLOYS

where v is the phonon frequency, B1, B2 and A are constants independent of v and G is the disorder parameter depending on the masses and radii of the constituent atoms. The lattice thermal resistivity W ¼ K1 obtained by Abeles [46] is given by WðxÞ ¼ Wp ðxÞ

)1 ( 1 5 tan U ½1ðtan1 U=UÞ2 þ 1þ a ð2:21Þ 9 U ½ð1 þ aÞ=5aU 4 ð1=3ÞU 2 ðtan1 U=UÞ þ 1

with 1 5 UðxÞ2 ¼ U0 ðxÞ2 1 þ a 9

ð2:22Þ

U0 ðxÞ2 ¼ A1 GðxÞWp ðxÞ1

ð2:23Þ

where

In Equations (2.21)–(2.23), Wp(x) is the lattice thermal resistivity of the crystal in which the disorder lattice is replaced by an ordered virtual crystal, a is a normal/Umklapp ratio (a ¼ B1/B2) and A1 is nearly constant within a group of ANB8N semiconductors. G(x) can be written as ( GðxÞ ¼ xð1xÞ

DM MðxÞ

2

" þ«

Dd

#)

dðxÞ2

ð2:24Þ

where DM ¼ MA MB, Dd ¼ dA dB, M(x) ¼ xMA þ (1 x)MB and d(x) ¼ xdA þ (1 x)dB (Mi and di (i ¼ A, B) are the masses and radii of the constituent atoms). « is regarded as a phenomenological, adjustable parameter. The first and second terms in the curly brackets in Equation (2.24) correspond to the contributions from the mass-defect and strain scatterings, respectively. Abeles’s model was used by Adachi [47,48] and Nakwaski [49] for several III–V alloys. Adachi [47] showed that for an AxB1xC alloy WðxÞ ¼ xWAC þ ð1xÞWBC þ xð1xÞCAB

ð2:25Þ

is essentially the same as Equation (2.21), where WAC and WBC are the binary thermal resistivities and CAB is a contribution arising from the lattice disorder (G) due to the random distribution of A and B atoms in the cation sublattice sites. Equation (2.25) is known as the Nordheim rule [50,51] and can be readily converted to the lattice thermal conductivity K KðxÞ ¼

1 1 ¼ WðxÞ xWAC þ ð1xÞWBC þ xð1xÞCAB

ð2:26Þ

In an AxB1xCyD1y quaternary alloy, not only should the A–B disorder due to the random distribution of the A and B atoms in the cation sublattice and the C–D disorder due to the random distribution of the C and D atoms in the anionic sublattice be taken into consideration, but also the fact that both the cation and anion sublattices are disordered as well. Neglecting the

THERMAL PROPERTIES

65

cation–anion interaction effect, we obtain Kðx;yÞ ¼ ¼

1 Wðx;yÞ

1 xyWAC þxð1yÞWAD þð1xÞyWBC þð1xÞð1yÞWBD þxð1xÞCAB þyð1yÞCCD ð2:27Þ

In doped semiconductors, the thermal conductivity can be given by the sum of the lattice and electronic contributions. In a metal, the electronic thermal conductivity K and electrical conductivity s at temperature T are related by the Wiedemann–Franz law K ¼ LTs

ð2:28Þ

r ¼ LTW

ð2:29Þ

or, equivalently

where L is the Lorenz number and r is the electrical resistivity. The thermal resistivity W as a function of x for CuxAu1x is shown in Figure 2.24. Cu–Au alloy is among the best studied of all metallic alloy systems. The solid and open circles represent the experimental data for the ordered (CuAu and Cu3Au) and disordered phases, 3 CuxAu1-x

W (cm K / W)

2

1

Cu3Au

CuAu 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.24 Thermal resistivity W as a function of x for CuxAu1x at 300 K. The solid circles represent the experimental data obtained from ordered alloys (CuAu and Cu3Au), while the open circles represent the data taken from disordered alloys. The solid and dashed lines are calculated from Equation (2.25) with CCuAu ¼ 8.15 cm K/W and with and without properly taking into account the alloy ordering effect at x ¼ 0.5 and 0.75 (CuAu and Cu3Au), respectively

66

PROPERTIES OF SEMICONDUCTOR ALLOYS

respectively. These data were obtained from various sources (e.g. Jacobsson and Sundqvist [52]). The solid and dashed lines are calculated from Equation (A.5) (Equation (2.25)) with CCuAu ¼ 8.15 cm K/W and with and without properly taking into account the ordering effect at x ¼ 0.5 and 0.75 (CuAu and Cu3Au), respectively. It is evident from Figure 2.24 that the ordered alloy data are much smaller than those estimated from Equation (2.25) (dashed line). The ordering in metallic alloy is, thus, found to greatly decrease W, irrespective of the ordered structure (CuAu ¼ L10 (tetragonal) or Cu3Au ¼ L12 (cubic)). Similarly, the electrical resistivity r of the ordered phase is much lower than that of the disordered phases (Figure 12.1). The ordering effect in semiconductor alloys was observed to occur spontaneously during epitaxial growth [53]. Kuan et al. [54] first observed an ordered phase (CuAu-I type) in an MOCVD-grown AlGaAs epilayer. Since the first finding of CuPt-type ordering in SiGe alloy [55], this type of ordering and others have also been reported in many III–V and II–VI semiconductor alloys (Section 1.3.2). However, no clear ordering effect on the carrier transport properties in semiconductor alloys has been observed. In the following, therefore, we pay no attention to the spontaneous ordering effect, except for CxSi1x with x ¼ 0.5 (3C-SiC). Since the lifetimes of the dominant phonons in semiconductor alloys are 100 ps, the frequency dependence of K would not be observable in experiments unless f > 1 GHz. However, the frequency-dependent K of Si0.4Ge0.6, Ga0.51In0.49P and Ga0.47In0.53As was clearly observed over a wide range of modulation frequencies 0.1 < f < 10 MHz and temperatures 88 < T < 300 K from time-dependent TR measurements [56]. The reduction in K at high frequencies was consistent with a model calculation assuming that phonons with mean free paths larger than the thermal penetration depth do not contribute to K as measured in the experiment. (b) Group-IV semiconductor alloy There has been no experimental or theoretical work on the thermal conductivity of CxSi1x. This is because of the low solubility of C in Si (6 106) [57]. In Figure 2.25 only the experimental K and W data for 3C-SiC (x ¼ 0.5) together with those for diamond and Si have been plotted [48]. Note that diamond and Si crystallize in the diamond structure, while 3C-SiC crystallizes in the zinc-blende structure. It is, therefore, considered that 3C-SiC is an ordered form of CxSi1x (x ¼ 0.5), or more succinctly, it is a compound, not an alloy. The solid lines in Figure 2.25 are calculated from Equations (2.25) and (2.26) without taking into account the contribution of alloy disorder (i.e. CCSi ¼ 0 cm K/W), while the dashed lines are obtained by assuming CCSi ¼ 15 cm K/W and properly taking into account the ordering effect at x ¼ 0.5. The diamond and Si values used in the calculation are taken from Table 2.2. In Figure 2.25, the thermal conductivity and resistivity of 3C-SiC can be satisfactorily interpreted by the linear interpolation scheme (CAB ¼ 0 cm K/W). It is also expected from Figure 2.25(b) that the alloying leads to a large increase in W due to increased disorder scattering (dashed line). Similarly, not only a large increase in W in doped Si [58,59], but also a decrease in W in isotopically enriched diamond [60–62] and Si [59,63] has been reported. Systematic work on the thermal conductivity of SixGe1x was carried out by Dismukes et al. [64] and the values they obtained for K and W are plotted in Figure 2.26. The solid lines represent the results calculated using Equations (2.25) and (2.26) with CSiGe ¼ 50 cm K/W [48]. The thermal resistivity markedly increased with alloying. The W value at x 0.5 is about 28 times as large as those of Si and Ge. Such a feature was motivated by desire to obtain increased performance for thermoelectric power conversion since the figure of merit for such a device

THERMAL PROPERTIES

67

Table 2.2 Room-temperature thermal conductivity K and resistivity W for some group-IV and III–V semiconductors, together with alloy disorder parameters Cab used in the calculation of K and W. d ¼ diamond; w ¼ wurtzite; zb ¼ zinc-blende Material

K (W/cm K)

W (cm K/W)

Cab (cm K/W)

Diamond (d) Si (d) Ge (d) AlN (w) AlP (zb) AlAs (zb) AlSb (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

22 1.56 0.60 3.19 0.90 0.91 0.57 1.95 0.77 0.45 0.36 0.45 0.68 0.30 0.175

0.045 0.64 1.67 0.31 1.1 1.10 1.75 0.51 1.30 2.22 2.78 2.22 1.47 3.3 5.71

CSiGe ¼ 50 CAlGa ¼ 32 CAlIn ¼ 15a CGaIn ¼ 72 CNP ¼ 36a CNAs ¼ 12a CNSb ¼ 10a CPAs ¼ 25 CPSb ¼ 16a CAsSb ¼ 91

a

Estimated from Equation (2.31)

25 K ( W/ cm K )

20

(a) CxSi1-x

15 3C -SiC

10 5 0 5

W (cm K / W)

4

(b)

3 2 1 0

3C -SiC 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.25 (a) Thermal conductivity K and (b) resistivity W versus x for CxSi1x at 300 K. The experimental data for diamond, Si and 3C-SiC (x ¼ 0.5) are taken from Table 2.2. The solid lines are calculated from Equations (2.25) and (2.26) without taking into account the contribution of alloy disorder (i.e. CCSi ¼ 0 cm K/W), while the dashed lines are obtained assuming CCSi ¼ 15 cm K/W and properly taking into account the alloy ordering effect at x ¼ 0.5 (3C-SiC). [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

68

PROPERTIES OF SEMICONDUCTOR ALLOYS

K (W/cm K)

2.0 1.5

(a)

SixGe1-x

1.0 0.5 0

W (cmK/W)

20 15

(b)

10 5 0

0

0.2

0.4

0.6

0.8

1

x

Figure 2.26 (a) Thermal conductivity K and (b) resistivity W versus x for SixGe1x at 300 K. The experimental data are taken from Dismukes et al. [64]. The solid lines are obtained from Equations (2.25) and (2.26) with CSiGe ¼ 50 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

application varies proportionally to W. One method of achieving a high value for W is by the use of a fine-grain SiGe technique, in which a decrease in thermal conductivity of up to 50% was attained by increasing grain-boundary scattering of phonons [65]. (c) III–V semiconductor alloy Figure 2.27 shows the thermal conductivity K versus x for (Al, Ga)–V ternaries: (a) wAlxGa1xN and (b) AlxGa1xAs [48]. The experimental data are taken for w-AlxGa1xN from Daly et al. [66] and Liu and Balandin [67] and for AlxGa1xAs from Afromowitz [68] and Pichardo et al. [69]. The solid lines represent the results calculated using Equation (2.26). The III–V binary data are taken from Table 2.2. The reduction in K from the binary value is much larger in w-AlxGa1xN than in AlxGa1xAs. However, these (Al, Ga)–V ternaries have the same disorder parameter CAlGa ¼ 32 cm K/W (solid lines). It was also found [66] that polycrystalline GaN has a thermal conductivity K, which is more than an order of magnitude lower than that of bulk GaN. It should be noted that the thermal conductivity K (or thermal resistivity W) is a quantity given by a second-rank symmetric tensor [25]. The wurtzite-type III–N semiconductors thus have two tensor components, K? and Kk. However, the difference between K? and Kk usually appears to be less than the experimental uncertainty at room temperature [70]. Figure 2.28 shows the thermal conductivity K versus x for (Ga, In)–V ternaries: (a) w-GaxIn1xN, (b) GaxIn1xAs and (c) GaxIn1xSb [48]. The experimental data in (a) are taken from Pantha et al. [71], in (b) from Abrahams et al. [72] and Arasly et al. [73] and in (c) from Magomedov et al. [74]. The solid lines in (a)–(c) represent the results calculated using Equation (2.26) with CGaIn ¼ 72 cm K/W. It should be noted that the InN value WInN ¼ 2.22 cm K/W used in the calculation corresponds to that for InN ceramics, not the bulk crystalline value. The dashed line in Figure 2.28(a) shows the result calculated using Equation (2.26) and a

THERMAL PROPERTIES 3. 5

69

1. 0 0. 9

(a) w-AlxGa1-xN

3. 0

(b) AlxGa1-xAs

0. 8

K (W/cm K )

2. 5

0. 7 0. 6

2. 0

0. 5 1. 5

0. 4 0. 3

1. 0

0. 2 0. 5 0

0. 1 0

0. 2

0. 4

0. 6

0. 8

1. 0

0

0

0. 2

0. 4

0. 6

0. 8

1. 0

x

x

Figure 2.27 Thermal conductivity K versus x for (Al, Ga)-based III–V ternaries at 300 K: (a) w-AlxGa1xN and (b) AlxGa1xAs. The experimental data in (a) are taken from Daly et al. [66] and Liu and Balandin [67] and in (b) from Afromowitz [68] and Pichardo et al. [69]. The solid lines are obtained from Equation (2.26) with CAlGa ¼ 32 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

2.5

0.5

0.5

K (W/cm K)

(a) w-GaxIn1-xN

(b) GaxIn1-xAs

(c) GaxIn1-xSb

2.0

0.4

0.4

1.5

0.3

0.3

1.0

0.2

0.2

0.5

0.1

0.1

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 2.28 Thermal conductivity K versus x for (Ga, In)-based III–V ternaries at 300 K: (a) w-GaxIn1xN, (b) GaxIn1xAs and (c) GaxIn1xSb. The experimental data in (a) are taken from Pantha et al. [71] (solid triangles), in (b) from Abrahams et al. [72] and Arasly et al. [73] (solid circles) and in (c) from Magomedov et al. [74] (solid circles). The solid lines in (a)–(c) are obtained from Equation (2.26) with CGaIn ¼ 72 cm K/W. The dashed line in (a) is also obtained from Equation (2.26) with a properly chosen value of WInN ¼ 0.5 cm K/W (open circle), instead of the ceramics InN value of WInN ¼ 2.22 cm K/W (solid line). [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

70

PROPERTIES OF SEMICONDUCTOR ALLOYS

properly chosen value of WInN ¼ 0.5 cm K/W, instead of the ceramics value WInN ¼ 2.22 cm K/W (solid line). The small WInN effect is remarkable only in the limited region x < 0.2. It is well known that dilute alloying of GaAs with InAs is a very effective technique for reducing the dislocation density of semiinsulating GaAs crystals grown by the liquidencapsulated Czochralski method. Ohmer et al. [75] studied the effect of the addition of a small quantity of InAs on the thermal properties of GaAs. They reported that for x ¼ 0.005 the thermal conductivity is reduced to 50% of the GaAs value. This region is in accordance with theory if the size difference is considered and combined coherently with the mass difference [76]. Values of K and W versus x for AlAsxSb1x are shown in Figures 2.29(a) and 2.29(b), respectively [48]. The experimental data are taken from Borca-Tasciuc et al. [77]. The solid lines are calculated from Equations (2.25) and (2.26) with CAsSb ¼ 91 cm K/W. The agreement between the calculated and experimental results was found to be very satisfactory. 1.0 K (W/cm K )

0.8

(a)

0.6

AlAsxSb1-x

0.4 0.2 0

W (cm K /W)

30 25

(b)

20 15 10 5 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.29 (a) Thermal conductivity K and (b) resistivity W versus x for AlAsxSb1x at 300 K. The experimental data are taken from Borca-Tasciuc et al. [77]. The solid lines are obtained from Equations (2.25) and (2.26) with CAsSb ¼ 91 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

The lattice thermal conductivity K versus x plots for III–(P, As) ternaries GaPxAs1x and InPxAs1x are shown in Figures 2.30(a) and 2.30(b), respectively [48]. The experimental data for GaPxAs1x are taken from Carlson et al. [78] and Maycock [79] and for InPxAs1x from Maycock [79] and Bowers et al. [80]. The solid lines represent the results calculated using Equation (2.26) with CPAs ¼ 25 cm K/W. The fit-determined disorder parameter CPAs ¼ 25 cm K/W is comparable to CAlGa ¼ 32 cm K/W, but much smaller than CGaIn ¼ 72 cm K/W and CAsSb ¼ 91 cm K/W. The K values of some III–V quaternaries are shown in Figure 2.31 [48]. The experimental data for AlxGa1xAsySb1y/GaSb are taken from Borca-Tasciuc et al. [77] and Both et al. [81], for GaxIn1xPyAs1y/InP from Both et al. [82] and for GaxIn1xAsySb1y/GaSb from Both et al. [81]. The theoretical curves in Figure 2.31 are obtained from Equation (2.27) with (a) CAlGa ¼ 32 cm K/W and CAsSb ¼ 91 cm K/W, (b) CGaIn ¼ 72 cm K/W and CPAs ¼ 25 cm K/W and

THERMAL PROPERTIES 1.0

1.0

K (W/cm K )

0.9

0.9

(a) GaPxAs1-x

0.8

0.8

0.7

0.7

0.6

0.6

0.5

0.5

0.4

0.4

0.3

0.3

0.2

0.2

0.1

0.1

0

71

0

0.2

0.4

0.6

0.8

1.0

0

(b) InPxAs1-x

0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 2.30 Thermal conductivity K versus x for (P, As)-based III–V ternaries at 300 K: (a) GaPxAs1x and (b) InPxAs1x. The experimental data in (a) are taken from Carlson et al. [78] and Maycock [79] and in (b) from Maycock [79] and Bowers et al. [80]. The solid lines are obtained from Equation (2.26) with CPAs ¼ 25 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

0.7

0.7

(a) AlxGa1-xAsySb1-y /GaSb

K (W/cm K)

0.6

0.7

(b) GaxIn1-xPyAs1-y /InP

0.6

0.5

0.5

0.5

0.4

0.4

0.4

0.3

0.3

0.3

0.2

0.2

0.2

0.1

0.1

0.1

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 y

(c) GaxIn1-xAsySb1-y /GaSb

0.6

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 2.31 Thermal conductivity K versus x or y for III–V quaternaries at 300 K: (a) AlxGa1xAsySb1y/GaSb, (b) GaxIn1xPyAs1y/InP and (c) GaxIn1xAsySb1y/GaSb. The experimental data for AlxGa1xAsySb1y/GaSb are taken from Borca-Tasciuc et al. [77] and Both et al. [81], for GaxIn1xPyAs1y/InP from Both et al. [82] and for GaxIn1xAsySb1y/GaSb from Both et al. [81]. The solid lines are calculated from Equation (2.27) with (a) CAlGa ¼ 32 cm K/W and CAsSb ¼ 91 cm K/W, (b) CGaIn ¼ 72 cm K/W and CPAs ¼ 25 cm K/W and (c) CGaIn ¼ 72 cm K/W and CAsSb ¼ 91 cm K/W. The dashed line in (c) represents the result calculated using Equation (2.27) with the introduction of the very small disorder parameters CGaIn ¼ 10 cm K/W and CAsSb ¼ 20 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

72

PROPERTIES OF SEMICONDUCTOR ALLOYS

(c) CGaIn ¼ 72 cm K/W and CAsSb ¼ 91 cm K/W. The disorder parameters Cab are obtained from the III–V ternary data analyses. The lattice-matching relationships between x and y are taken from Tables 1.9 and 1.10. The agreement between the experimental and calculated data in Figures 2.31(a) and 2.31(b) is very good and successfully explains the composition dependence of K in the alloys. It should be noted, however, that the calculation in Figure 2.31(c) produces a K value considerably lower than the experimental value. The input of very small Cab values into Equation (2.27) improves the fit very well; however, the endpoint ternary K value (InAs0.91Sb0.09) becomes very large and the binary K value (GaSb) very small, compared with the generally accepted values. The dashed line in Figure 2.31(c) shows an example of such a calculation. Putting CGaIn ¼ 10 cm K/W and CAsSb ¼ 20 cm K/W into Equation (2.27), we obtain K ¼ 0.30 W/cm K for x ¼ 0 (InAs0.91Sb0.09) and 0.25 W/cm K for x ¼ 1.0 (GaSb), which are far from the generally accepted values. If the endpoint K values and Cab are available, the lattice thermal conductivity and its dependence on alloy composition can easily be calculated from Equation (2.26) or Equation (2.27). At the limit of weak scattering, the disorder parameter G in Equation (2.24) can be simply written as X Mi M 2 G¼ ci ð2:30Þ M i where ci is the fractional concentration of the ith species, Mi is the atomic mass of the ith species is the average atomic mass. and M Figure 2.32 plots the obtained Cab values versus G [48]. It can be seen that Cab decreases with the increase in G. The solid line represents the least-squares fit of the III–V ternaries given by (Cab in cm K/W) Cab ¼

Cαβ (cm K / W)

102

G 7:7

0:90

ð2:31Þ

As-Sb Si-Ge

Ga-In

Al-Ga P-As Cu-Au

101

10-1 Γ

Figure 2.32 Cab versus G determined for some group-IV binary and III–V ternary alloys and metallic Cu–Au alloy at 300 K. The solid line represents the least-squares fit (III–V ternary data) using Equation (2.31). [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

THERMAL PROPERTIES

73

Using this expression, the unknown Cab value can be estimated. For example, G of the cationic disorder system i ¼( Al, In) in Equation (2.30) is 0.384. Introducing this value into Equation (2.31), we obtain CAlIn ¼ 15 cm K/W. Figure 2.33 shows the lattice thermal conductivity as a function of x for (a) GaxIn1xP and (b) GaAsxSb1x [48]. No experimental data are available for these alloys. The solid lines are calculated from Equation (2.26) with CGaIn ¼ 72 cm K/W in (a) and CAsSb ¼ 95 cm K/W in (b). As expected, the calculated K value markedly decreases with alloying and exhibits a minimum at x 0.5. 1. 0

0. 5

K (W/cm K)

(a) GaxIn1-xP

(b) GaAsxSb1-x

0. 8

0. 4

0. 6

0. 3

0. 4

0. 2

0. 2

0. 1

0

0 0

0. 2

0. 4

0. 6

0. 8

1. 0

0

0. 2

0. 4

x

0. 6

0. 8

1. 0

x

Figure 2.33 Thermal conductivity K versus x for some III–V ternaries at 300 K: (a) GaxIn1xP and (b) GaAsxSb1x. These values were estimated from Equation (2.26) with CGaIn ¼ 72 cm K/W (a) and CAsSb ¼ 95 cm K/W (b) (solid lines). The solid circles represent the experimental endpoint binary data. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

In an AxByCzD (ABxCyDz) quaternary alloy, the lattice thermal conductivity K can be written as Kðx; y; zÞ ¼

1 1 ¼ Wðx; y; zÞ xWAD þ yWBD þ zWCD þ xyCAB þ xzCAC þ yzCBC

ð2:32Þ

with xþyþz ¼ 1

or z ¼ 1xy

ð2:33Þ

Since the thermal conductivity or resistivity in Equation (2.32) is specified in terms of the alloy composition x, y and z only, K or W of a quaternary alloy with arbitrary composition can easily be calculated. For example, the thermal conductivity of AlxGayIn1xyN can be estimated from (in W/cm K) KAlGaInN ðx; y; zÞ ¼

1 3:19x þ 1:95y þ 0:45z þ 32xy þ 15xz þ 72yz

ð2:34Þ

74

PROPERTIES OF SEMICONDUCTOR ALLOYS

Similarly, the K values for (AlxGa1x)0.53In0.47P/GaAs and (AlxGa1x)0.48In0.52As/InP can be estimated, as shown in Figure 2.34 [48]. The disorder parameters Cab used are taken from Table 2.2. The lattice-matching relationships between x and y for these quaternaries are taken from Table 1.11. 0.30

0.30

K (W/cm K)

(AlxGa1-x)0.53In0.47P/GaAs

(AlxGa1-x)0.48In0.52As/InP

0.25

0.25

0.20

0.20

0.15

0.15

0.10

0.10

0.05

0.05 (a)

0

0

0.2

0.4

0.6 x

0.8

(b) 1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.34 Thermal conductivity K versus x for some III–V quaternaries at 300 K: (a) (AlxGa1x)0.53In0.47P/GaAs and (b) (AlxGa1x)0.48In0.52As/InP. These values were estimated from Equation (2.32) with CAlGa ¼ 32 cm K/W, CAlIn ¼ 15 cm K/W and CGaIn ¼ 72 cm K/W. [Reprinted with permission from S. Adachi, J. Appl. Phys. 102, 3502 (2007). Copyright (2007), American Institute of Physics]

(d) II–VI semiconductor alloy Ioffe and Ioffe [83] reported the thermal conductivity of ZnTe–CdTe, CdSe–HgSe, ZnSe–ZnTe, HgSe–HgTe, ZnSe–CdTe and ZnTe–CdSe alloys. Each of the starting materials was crushed into a fine powder, carefully blended in the required proportions, compressed under a pressure of 2–5 t/cm2 at a temperature of about 300 C and then repeatedly annealed at higher temperatures until a stable value of thermal conductivity was attained. All the experimental data showed a marked decrease in thermal conductivity with alloying. Because of the ceramic-like nature of the samples, their absolute values may be much smaller than those of the bulk crystalline materials. Aliev et al. [84] have reported the temperature dependence of K for CdxHg1xTe with x ¼ 00.2. These results are shown in Figure 2.35. The data give a maximum K near 8 K. In the temperature range from 10 to 100 K, HgTe (x ¼ 0) has a thermal conductivity proportional to T 1.2. The alloys with x > 0 have lower thermal conductivities and the temperature exponents are also less. The experimentally determined exponents for various non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Table 2.9 of Adachi [25]. The thermal conductivities K for ZnxHg1xTe and CdxHg1xTe and their melts were reported by Sha et al. [85] and Su [86], respectively. These data were determined from the experimental diffusivities and theoretical specific heats (Section 2.5.2).

THERMAL PROPERTIES

75

Figure 2.35 Thermal conductivity K for CdxHg1xTe with x ¼ 0, 0.05, 0.1 and 0.2. [Reprinted from Sov. Phys Solid State 2, 719 (1960)] The solid line represents the exponential relationship, K / T 1.2

2.5.2 Thermal Diffusivity (a) General considerations The thermal diffusivity D can be obtained from the thermal conductivity K by means of the definition D¼

K Cp g

ð2:35Þ

where Cp and g represent the specific heat at constant pressure and crystal density, respectively. Thermal diffusivity D is measured in cm2/s. (b) Alloy value Figure 2.36 shows the inverse plots of D versus x for (a) CxSi1x and (b) AlxGa1xAs. The endpoint data are indicated by the open circles. The experimental data for 3C-SiC is also shown in Figure 2.36(a) by the solid circle. The solid line in Figure 2.36(b) is obtained from Equation (2.35) using the K and Cp values in Table 2.2 (Equation (2.26)) and Equation (2.10), respectively. The inverse thermal diffusivity D1 of 3C-SiC is found to be well interpreted by the linear interpolation between the endpoint data. Figure 2.37 shows the plot of K and D versus x for (GaAs)x(InP)1x quaternary. The K values are obtained from (in W/cm K) KðGaAsÞðInPÞ ðxÞ ¼

1 2:22x þ 1:47ð1xÞ þ 72xð1xÞ þ 25xð1xÞ

ð2:36Þ

76

PROPERTIES OF SEMICONDUCTOR ALLOYS

D-1 (s/cm2)

1.5 1.2

(a) CxSi1-x

3C-SiC

0.9 0.6 0.3 0 20

D-1 (s/cm2)

16 12 8 (b) AlxGa1-xAs

4 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.36 Inverse thermal diffusivity D versus x for (a) CxSi1x and (b) AlxGa1xAs at 300 K. The solid line in (a) represents the linear interpolation result between the endpoint data (open circles)

K (W/cm K)

0.8 0.6

(a)

0.4 (GaAs)x(InP)1-x 0.2 0 0.5

D (cm2/s)

0.4

(b)

0.3 0.2 0.1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 2.37 (a) Thermal conductivity K and (b) diffusivity D versus x for (GaAs)x(InP)1x quaternary at 300 K. The solid circles represent the experimental endpoint binary data

The Cp values used in the calculation of D are taken from Equation (2.9), while g is interpolated between GaAs and InP.

REFERENCES [1] H. St€ohr and W. Klemm, Z. Anorg. Allg. Chem. 241, 305 (1939). [2] T. Soma, Phys. Status Solidi B 111, K23 (1982).

THERMAL PROPERTIES [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34] [35] [36] [37] [38] [39] [40] [41]

77

L. M. Foster and J. F. Woods, J. Electrochem. Soc. 118, 1175 (1971). G. B. Stringfellow, J. Phys. Chem. Solids 33, 665 (1972). M. B. Panish and M. Ilegems, Prog. Solid State Chem. 7, 39 (1972). S. Adachi, J. Appl. Phys. 58, R1 (1985). N. A. El-Masry, E. L. Piner, S. X. Liu, and S. M. Bedair, Appl. Phys. Lett. 72, 40 (1998). D. Doppalapudi, S. B. Basu, K. F. Ludwig, Jr., and T. D. Moustakas, J. Appl. Phys. 84, 1389 (1998). T. Saito and Y. Arakawa, Phys. Rev. B 60, 1701 (1999). T. Takeyama, M. Yuri, K. Itoh, T. Baba, and J. S. Harris, Jr., J. Appl. Phys. 88, 1104 (2000). L. K. Teles, J. Furthm€uller, L. M. R. Scolfaro, J. R. Leite, and F. Bechstedt, Phys. Rev. B 62, 2475 (2000). M. Ferhat and F. Bechstedt, Phys. Rev. B 65, 075213 (2002). J. Adhikari and D. A. Kofke, J. Appl. Phys. 95, 4500 (2004). S. Y. Karpov, N. I. Podolskaya, I. A. Zhmakin, and A. I. Zhmakin, Phys. Rev. B 70, 235203 (2004). C. K. Gan, Y. P. Feng, and D. J. Srolovitz, Phys. Rev. B 73, 235214 (2006). S. Raghavan, J. P. Hajra, G. N. K. Iyengar, and K. P. Abraham, Thermochim. Acta 189, 151 (1991). V. L. Solozhenko, A. N. Baraov, and V. Z. Turkevich, Solid State Commun. 138, 534 (2006). J. Steininger, A. J. Strauss, and R. F. Brebrick, J. Electrochem. Soc. 117, 1305 (1970). A. G. Fischer and W. H. Fonger, Report No. 3 (1965), Contract No. AF 19 (628)-3866, US Air Force, Cambridge Research Laboratories, Bedford, Mass., USA. A. J. Strauss and J. Steininger, J. Electrochem. Soc. 117, 1420 (1970). J. Steininger and A. J. Strauss, J. Cryst. Growth 13/14, 657 (1972). K. Ohata, J. Saraie, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1198 (1973). D. A. Wood, K. D. Rogers, D. W. Lane, G. J. Conibeer, and D. Parton, J. Mater. Sci. Lett. 17, 1511 (1998). See, T. C. Harman, in Physics and Chemistry of II–VI Compounds (edited by M. Aven and J. S. Prener), North-Holland, Amsterdam, 1967, p. 767. S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. H.-M. Kagaya, Y. Kitani, and T. Soma, Solid State Commun. 58, 399 (1986). A. N. N. Sirota, A. M. Antyukhov, and V. A. Fedorov, Sov. Phys. Dokl. 26, 701 (1981). A. N. N. Sirota, A. M. Antyukhov, V. V. Novikov, and A. A. Sidorov, Sov. Phys. Dokl. 27, 754 (1982). S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties. World Scientific, Singapore, 1994. N. N. Sirota, N. P. Gavaleshko, V. V. Novikova, A. V. Novikova, and V. M. Frasunyak, Russ. J. Phys. Chem. 64, 603 (1990). M. Gambino, V. Vassiliev, and J. P. Bros, J. Alloys Compounds 176, 304 (1987). H. Maleki and L. R. Holland, in Properties of Narrow Gap Cadmiun-based Compounds, EMIS Datareviews Series No. 10 (edited by P. Capper), INSPEC, London, 1994, p. 48. C. G. Shirley, Acta Crsyt. A 31, 853 (1975). V. N. Nikiforov and V. G. Sredin, Rus. Phys. J. 49, 337 (2006). V. V. Zhdanova, M. G. Kakna, and T. Z. Samadashvili, Izv. Akad. Nauk. SSSR Neorg. Mater. 3, 1263 (1967). N. S. Takahashi, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 3. _ J. Bak-Misiuk, J. Domagała, W. Paszkowicz, J. Trela, Z. R. Zytkiewicz, M. Leszczy nski, K. Reginski, J. Muszalski, J. H€artwig, and M. Ohler, Acta Phys. Polonica A 91, 911 (1997). I. Kudman and R. J. Paff, J. Appl. Phys. 43, 3760 (1972). M. Leszczynski, A. Kulik, and P. Ciepielewski, Phys. Status Solidi A 119, 495 (1990). M. E. Straumanis, J.-P. Krumme, and M. Rubenstein, J. Electrochem. Soc. 114, 640 (1967). S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992.

78

PROPERTIES OF SEMICONDUCTOR ALLOYS

[42] V. N. Bessolov, S. G. Konnikov, V. E. Umanskii, and Y. P. Yakoviev, Sov. Phys. Tech. Phys. 28, 257 (1983). [43] D. Bagot, R. Granger, and S. Rolland, Phys. Status Solidi B 177, 295 (1993). [44] J. R. Kim, R. M. Park, and K. S. Jones, Mater. Res. Soc. Symp. Proc. 340, 475 (1994). [45] W.-T. Kim, Phys. Rev. B 59, 4572 (1999). [46] B. Abeles, Phys. Rev. 131, 1906 (1963). [47] S. Adachi, J. Appl. Phys. 54, 1844 (1983). [48] S. Adachi, J. Appl. Phys. 102, 063502 (2007). [49] W. Nakwaski, J. Appl. Phys. 64, 159 (1988). [50] L. Nordheim, Ann. Phys. 401, 607 (1931). [51] L. Nordheim, Ann. Phys. 401, 641 (1931). [52] P. Jacobsson and B. Sundqvist, J. Phys. Chem. Solids 49, 441 (1988). [53] A. Mascarenhas, Spontaneous Ordering in Semiconductor Alloys, Kluwer Academic, New York, 2002. [54] T. S. Kuan, T. F. Kuech, W. I. Wang, and E. L. Wilkie, Phys. Rev. Lett. 54, 201 (1985). [55] A. Ourmazd and J. C. Bean, Phys. Rev. Lett. 55, 765 (1985). [56] Y. K. Koh and D. G. Cahill, Phys. Rev. B 76, 075207 (2007). [57] E. T. Croke, A. T. Hunter, C. C. Ahn, T. Laursen, D. Chandrasekhar, A. E. Bair, D. J. Smith, and J. W. Mayer, J. Cryst. Growth 175–176, 486 (1997). [58] M. Asheghi, K. Kurabayashi, R. Kasnavi, and K. E. Goodson, J. Appl. Phys. 91, 5079 (2002). [59] D. G. Cahill and F. Watanabe, Phys. Rev. B 70, 235322 (2004). [60] T. R. Anthony, W. F. Banholzer, J. F. Fleischer, L. Wei, P. K. Kuo, R. L. Thomas, and R. W. Pryor, Phys. Rev. B 42, 1104 (1990). [61] D. G. Onn, A. Witek, Y. Z. Wie, T. R. Anthony, and W. F. Banholzer, Phys. Rev. Lett. 68, 2806 (1992). [62] J. R. Olson, R. O. Pohl, J. W. Vandersande, A. Zoltan, T. R. Anthony, and W. F. Banholzer, Phys. Rev. B 47, 14850 (1993). [63] W. S. Capinski, H. J. Maris, E. Bauser, I. Silier, M. Asen-Palmer, T. Ruf, M. Cardona, and E. Gmelin, Appl. Phys. Lett. 71, 2109 (1997). [64] J. P. Dismukes, L. Ekstrom, E. F. Steigmeier, I. Kudman, and D. S. Beers, J. Appl. Phys. 35, 2899 (1964). [65] C. B. Vining, W. Laskow, J. O. Hanson, R. R. Van der Beck, and P. D. Gorsuch, J. Appl. Phys. 69, 4333 (1991). [66] B. C. Daly, H. J. Maris, A. V. Nurmikko, M. Kuball, and J. Han, J. Appl. Phys. 92, 3820 (2002). [67] W. Liu and A. A. Balandin, Appl. Phys. Lett. 85, 5230 (2004). [68] M. A. Afromowitz, J. Appl. Phys. 44, 1292 (1973). [69] J. L. Pichardo, J. J. Alvarado-Gil, A. Cruz, J. G. Mendoza, and G. Torres, J. Appl. Phys. 87, 7740 (2000). [70] G. A. Slack and S. B. Austerman, J. Appl. Phys. 42, 4713 (1971). [71] B. N. Pantha, R. Dahal, J. Li, J. Y. Lin, H. X. Jiang, and G. Pomrenko, Appl. Phys. Lett. 92, 042112 (2008). [72] M. S. Abrahams, R. Braunstein, and F. D. Rosi, J. Phys. Chem. Solids 10, 204 (1959). [73] D. G. Arasly, R. N. Ragimov, and M. I. Aliev, Sov. Phys. Semicond. 24, 225 (1990). [74] Y. B. Magomedov, N. L. Kramynina, and S. M. Ismaılov, Sov. Phys. Solid State 34, 1486 (1992). [75] M. C. Ohmer, W. C. Mitchel, G. A. Graves, D. E. Holmes, H. Kuwamoto, and P. W. Yu, J. Appl. Phys. 64, 2775 (1988). [76] F. Szmulowicz, F. L. Madarasz, P. G. Klemens, and J. Diller, J. Appl. Phys. 66, 252 (1989). [77] T. Borca-Tasciuc, D. W. Song, J. R. Meyer, I. Vurgaftman, M.-J. Yang, B. Z. Nosho, L. J. Whitman, H. Lee, R. U. Martinelli, G. W. Turner, M. J. Manfra, and G. Chen, J. Appl. Phys. 92, 4994 (2002). [78] R. O. Carlson, G. A. Slack, and S. J. Silverman, J. Appl. Phys. 36, 505 (1965). [79] P. D. Maycock, Solid-State Electron. 10, 161 (1967). [80] R. Bowers, J. E. Bauerle, and A. J. Cornish, J. Appl. Phys. 30, 1050 (1959).

THERMAL PROPERTIES [81] [82] [83] [84] [85] [86]

79

W. Both, A. E. Bochkarev, A. E. Drakin, and B. N. Sverdlov, Cryst. Res. Technol. 24, K161 (1989). W. Both, V. Gottschalch, and G. Wagner, Cryst. Res. Technol. 21, K85 (1986). A. V. Ioffe and A. F. Ioffe, Sov. Phys. Solid State 2, 719 (1960). S. A. Aliev, T. G. Gadzhive, and R. I. Selim-zade, Sov. Phys. Solid State 31, 346 (1989). Y.-G. Sha, C.-H. Su, K. Mazuruk, and S. L. Lehoczky, J. Appl. Phys. 80, 752 (1996). C.-H. Su, J. Cryst. Growth 78, 51 (1986).

3 Elastic Properties 3.1 ELASTIC CONSTANT 3.1.1 General Considerations The second-order elastic stiffness [C] and compliance tensors [S] are defined by the generalized Hooke’s law: ½X ¼ ½C½e or ½e ¼ ½S½X, where [X] and [e] are, respectively, the elastic stress and strain tensors which have six components. The elastic tensors [C] and [S] are second-order fourth-rank and have symmetric 6 6 components. Their explicit tensor forms are given in Adachi [1]. We present in Tables 3.1–3.3 the elastic stiffness and compliance constants for a number of group-IV, III–V and II–VI semiconductors used for obtaining alloy values.

3.1.2 Room-temperature Value (a) Group-IV semiconductor alloy Figure 3.1 shows the elastic constants Cij of the metallic alloy Cu–Au. The solid and open circles represent the experimental ordered (CuAu3 and Cu3Au) and disordered phase data, respectively, gathered from various sources. The solid lines show the linear interpolation values between Au and Cu. No clear ordering effect can be found in the elastic properties of the metallic alloy. Figure 3.2 shows the plots of experimental Cij data for 3C-SiC (x ¼ 0.5), together with those for diamond and Si. Note that 3C-SiC crystallizes in the zinc-blende structure and is a compound, not an alloy. The solid lines show the linear interpolation between diamond and Si. Because of the extremely large Cij values of diamond, the linearly interpolated SiC values deviate considerably from the experimental values. Mendik et al. [2] determined the elastic constants of a relaxed Si0.49Ge0.51 film using Brillouin scattering and his data are shown in Figure 3.3, together with those of Si and Ge. The alloy value can be safely estimated using the linear interpolation scheme. (b) III–V semiconductor alloy Only a few reports of the direct measurement of elastic constants are available for III–V semiconductor alloys. The elastic constants Cij of GaxIn1xSb have been determined using a pulse echo method [3]. Figure 3.4 shows these results. The linearly interpolated values are shown by the solid lines and the experimental data are in good agreement with the linear interpolation results. Figure 3.5 shows the elastic constants Cij versus y or x for (a) GaxIn1xPyAs1y/InP and (b) (AlxGa1x)0.53In0.47P/GaAs. The solid circles show the endpoint data determined by Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

82

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 3.1 Elastic stiffness Cij and compliance constants Sij for a number of cubic group-IV, III–V and II–VI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

Cij (1011 dyn/cm2)

Material

Sij (1012 cm2/dyn)

C11

C12

C44

S11

S12

S44

107.9 16.564 12.870 6.90 39.0

12.4 6.394 4.770 2.93 14.2

57.8 7.951 6.670 3.62 25.6

0.0949 0.7691 0.9718 1.94 0.318

0.00978 0.2142 0.2628 0.578 0.085

0.1730 1.2577 1.499 2.76 0.391

IV

Diamond (d) Si (d) Ge (d) Sn (d)a 3C-SiC (zb)

III–V

BN (zb) BP (zb) BAs (zb)b AlN (zb)b AlP (zb)b AlAs (zb) AlSb (zb) GaN (zb)b GaP (zb) GaAs (zb) GaSb (zb) InN (zb)b InP (zb) InAs (zb) InSb (zb)

82.0 31.5 27.9 31.5 15.0 11.93 8.769 29.1 14.050 11.88 8.838 19.2 10.22 8.329 6.608

19.0 10 12.0 15.0 6.42 5.72 4.341 14.8 6.203 5.38 4.027 7.30 5.73 4.526 3.531

48.0 16 11.3 18.5 6.11 5.72 4.076 15.8 7.033 5.94 4.320 9.35 4.42 3.959 3.027

0.134 0.37 0.484 0.458 0.897 1.216 1.697 0.523 0.9756 1.173 1.583 0.659 1.639 1.945 2.410

0.025 0.09 0.145 0.148 0.269 0.394 0.5618 0.176 0.2988 0.366 0.4955 0.182 0.589 0.6847 0.8395

0.208 1.00 0.885 0.541 1.64 1.748 2.453 0.633 1.422 1.684 2.315 1.07 2.26 2.526 3.304

II–VI

BeS (zb)b BeSe (zb)b BeTe (zb)b MgO (rs) MgS (zb)b MgSe (zb)b MgTe (zb)b ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

12.3 11.0 8.87 29.4 8.88 7.58 5.28 10.2 8.57 7.15 7.70 6.67 5.35 8.13 6.08 5.32

7.30 6.66 5.54 9.3 5.53 4.86 3.66 6.46 5.07 4.08 5.39 4.63 3.69 6.22 4.46 3.68

5.69 5.03 3.86 15.5 3.87 3.17 1.93 4.46 4.05 3.11 2.36 2.23 2.02 2.64 2.23 2.08

1.47 1.66 2.16 0.401 2.16 2.64 4.38 1.95 2.09 2.39 3.07 3.48 4.27 3.65 4.34 4.33

0.55 0.63 0.83 0.096 0.83 1.03 1.79 0.76 0.78 0.85 1.26 1.42 1.74 1.58 1.84 1.77

1.76 1.99 2.59 0.647 2.58 3.15 5.18 2.25 2.47 3.25 4.24 4.48 4.95 3.79 4.49 4.80

a b

Obtained from an analysis of the phonon dispersion curves at 90 K Calculated or estimated

ELASTIC PROPERTIES

83

Table 3.2 Elastic stiffness constant Cij for a number of hexagonal group-IV, III–V and II–VI semiconductors at 300 K (in 1011 dyn/cm2). w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)) System

Material

C11

C12

IV

2H-SiC (w)b

50.1

11.1

III–V

BN (h) AlN (w) GaN (w) InN (w)

52.0 41.0 37.3 19.0

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

46.1 20.9 12.2 8.65 7.41

a b

C33

C44

C66a

5.2

55.3

16.3

19.5

43.1 14.0 14.1 10.4

37.0 10.0 8.0 12.1

42.4 39.0 38.7 18.2

6.5 12.0 9.4 0.99

4.5 13.5 11.6 4.3

12.6 12.0 5.8 5.40 4.52

8.85 10.4 4.2 4.73 3.9

49.2 21.8 13.8 9.44 8.43

14.8 4.41 2.87 1.50 1.34

16.8 4.45 3.2 1.63 1.45

C13

C66 ¼ 1/2(C11 C12) Assuming that the 2H-SiC values are the same as those for 6H-SiC within experimental error

Table 3.3 Elastic compliance constant Sij for a number of hexagonal group-IV, III–V and II–VI semiconductors at 300 K (in 1012 cm2/dyn). w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)) System

Material

IV

S12

S13

S33

2H-SiC (w)b

0.211

0.045

0.016

0.184

0.614

0.512

III–V

BN (h) AlN (w) GaN (w) InN (w)

0.726 0.285 0.320 0.957

0.398 0.085 0.112 0.206

0.286 0.051 0.043 0.499

0.735 0.283 0.276 1.21

1.54 0.833 1.06 10.1

2.25 0.740 0.864 2.33

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

0.240 0.782 1.10 2.08 2.32

0.060 0.345 0.45 1.00 1.12

0.032 0.210 0.20 0.54 0.55

0.215 0.664 0.86 1.60 1.69

0.677 2.24 3.48 6.66 7.47

0.600 2.254 3.10 6.16 6.88

a b

S44

S66a

S11

S66 ¼ 2(S11 S12) Assuming that the 2H-SiC values are the same as those for 6H-SiC within experimental error

Brillouin scattering for Ga0.47In0.53As [4] and Ga0.53In0.47P [5]. Since the lattice-matched quaternaries have thesame lattice constants over the entire composition range (aInP ¼ 5.8690 A or aGaAs ¼ 5.65330 A), their elastic constants are not expected to show strong dependence on the alloy composition [1]. The solid lines in Figures 3.5(a) and 3.5(b) represent the results calculated using Equations (A.6) and (A.8), respectively.

84

PROPERTIES OF SEMICONDUCTOR ALLOYS

C44 (GPa)

C12 (GPa)

C11 (GPa)

CuAu3 (LI2)

220 200 180 160 140 180 160 140 120 100 100 80 60 40 20 0

Cu3Au (LI2)

(a) Cux Au1-x (b)

(c) 0.2

0.4

x

0.6

0.8

1.0

Figure 3.1 Elastic constants Cij of Cu–Au. The solid and open circles represent the experimental ordered (LI2 type) and disordered alloy data, respectively. The solid lines show the linear interpolation results between Au and Cu

CxSi1-x (a)

C12 (GPa)

C11 (GPa)

1200 900 600 300 0 180 150 120 90 60 30 0 800 600 400 200 0 0

C44 (GPa)

3C-SiC

(b)

(c) 0.2

0.4

x

0.6

0.8

1.0

Figure 3.2 Elastic constants Cij of CxSi1x at 300 K. The solid circles represent the 3C-SiC data (x ¼ 0.5). The solid lines show the linear interpolation results between the endpoint elemental data

(c) II–VI semiconductor alloy The elastic constant C11 of MBE-BexZn1xSe on GaAs(100) has been determined using Brillouin scattering [6]. Figure 3.6 shows these results. The BeSe value is estimated from the simple Cij–a (lattice parameter) relationship described in Adachi [1]. The solid line is linearly interpolated between the endpoint binary data. The experimental data in Figure 3.6 suggest an upward bowing. Peiris et al. [6] determined C11 from the sound velocities vs by measuring

ELASTIC PROPERTIES

85

C11 (GPa)

180 150

SixGe1-x

120

(a)

C12 (GPa)

90 80 60 40

(b)

C44 (GPa)

20 100 80 60 40 0

(c) 0.2

0.4

x

0.6

0.8

1.0

Figure 3.3 Elastic constants Cij of SixGe1x at 300 K. The experimental data (x ¼ 0.49) are taken from Mendik et al. [2]. The solid lines show the linear interpolation results between the endpoint elemental data C11 (GPa)

90 80

GaxIn1-xSb

70

(a)

C44 (GPa)

C12 (GPa)

60 45 40 35 30 50 45 40 35 30 25

(b)

(c) 0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.4 Elastic constants Cij of GaxIn1xSb at 300 K. The experimental data are taken from Galibert and Bougnot [3]. The solid lines show the linear interpolation results between the endpoint binary data

frequency shift Dv of the Brillouin components using the relationship Dv ¼ 2vL n

vs u sin 2 c

ð3:1Þ

where vL is the frequency of the incident laser radiation, n is the refractive index of the material, c is the speed of light in vacuum and u is the scattering angle (180 ). Using a prism coupler technique, they also determined n for BexZn1xSe. Figure 3.7 shows the elastic constants Cij versus x for ZnxCd1xTe. The experimental data are taken from Andrusiv et al. [7] (x ¼ 0.35, 0.57 and 0.71), from Maheswaranathan et al. [8]

PROPERTIES OF SEMICONDUCTOR ALLOYS

C44 (GPa)

C12 (GPa)

C11 (GPa)

86

130 120 110 100 90 70

130 120 110 100 90 70

(a) GaxIn1-xPyAs1-y /InP

60

60

50

50

40 70

40 70

60

60

50

50

40

0

0.2

0.4

y

0.6

0.8

40

1.0

(b) (AlxGa1-x)0.53In0.47P/GaAs

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.5 Elastic constants Cij versus y or x for (a) GaxIn1xPyAs1y/InP and (b) (AlxGa1x)0.53 In0.47P/GaAs at 300 K. The open circles in (a) represent the InP data, while the solid circles in (a) and (b) show the endpoint ternary data taken from Carlotti et al. [4] (Ga0.47In0.53As) and Hassine et al. [5] (Ga0.53In0.47P), respectively. The solid lines show the linear interpolation results of Equations (A.6) and (A.8)

140

C11 (GPa)

120 100 80 60 0

Bex Zn1-xSe 0.2

0.4

x

0.6

0.8

1.0

Figure 3.6 Elastic constant C11 of MBE-grown BexZn1xSe on GaAs(1 0 0) at 300 K. The experimental data are taken from Peiris et al. [6]. The solid line shows the linear interpolation result between the endpoint binary data

(x ¼ 0.48) and from Queheillalt and Wadley [9] (x ¼ 0.04). These data are in agreement with the linearly interpolated values within experimental accuracy.

3.1.3 External Perturbation Effect (a) Temperature effect Only a few reports are available on the temperature dependence of Cij for III–V and II–VI alloys [3,7,9]. Figure 3.8 shows the linearly interpolated dCij/dT versus y for GaxIn1xPyAs1y/ InP calculated from Equation (A.6). The binary values used are taken from Table 3.8 in Adachi [1].

ELASTIC PROPERTIES

87

C11 (GPa)

80 ZnxCd1-xTe

70 60

(a)

C44 (GPa)

C12 (GPa)

50 45 40 35 30 35 30 25 20 15

(b)

(c) 0

0.2

0.4

x

0.6

0.8

1.0

dC11 /dT dC44 /dT dC12 /dT (107 dyn/cm2 K) (107 dyn/cm2 K) (107 dyn/cm2 K)

Figure 3.7 Elastic constants Cij versus x for ZnxCd1xTe at 300 K. The experimental data are taken from Andrusiv et al. [7] (x ¼ 0.35, 0.57 and 0.71), from Maheswaranathan et al. [8] (x ¼ 0.48) and from Queheillalt and Wadley [9] (x ¼ 0.04). The solid lines show the linear interpolation results between the endpoint binary data

-12 -14

GaxIn1-xPyAs1-y /InP

-16

(a)

-18 -4 (b)

-6 -8 -10 -2 -4 -6 -8 -10 0

(c) 0.2

0.4

y

0.6

0.8

1.0

Figure 3.8 Linearly interpolated dCij/dT versus y for GaxIn1xPyAs1y/InP at 300 K. The binary dCij/dT data used in the calculation (Equation (A.6)) are taken from Adachi [1]

The temperature-dependent Cij values of ZnxCd1xTe have been determined from 78 to 300 K [7] and from 300 up to 1413 K [9]. The solid circles in Figure 3.9 show the dCij/dT data for ZnxCd1xTe (x ¼ 0.04) [9]. The endpoint data taken from Table 3.8 in Adachi [1] are also shown by the open circles. The x ¼ 0.04 data are found to largely deviate from the linearly interpolated values. The temperature-dependent Cij values for GaxIn1xSb (x ¼ 0.78–0.95) were also measured using the pulse echo method between 4 and 300 K [3].

PROPERTIES OF SEMICONDUCTOR ALLOYS dC44 /dT dC12/dT dC11 /dT (107 dyn/cm2 K) (107 dyn/cm2 K) (107 dyn/cm2 K)

88

-6 -8 -10 -12 -14 -16 -4 -6 -8 -10 -12 0 -2 -4 -6 -8 0

(a)

ZnxCd1-xTe

(b)

(c)

0.2

0.4

0.6

x

0.8

1.0

Figure 3.9 dCij/dT versus x for ZnxCd1xTe at 300 K. The data represented by solid circles are taken from Queheillalt and Wadley [9] (x ¼ 0.04), while the open circles represent the endpoint binary data [1]

(b) Pressure effect

dC12 /dp

dC11 /dp

The pressure coefficient dCij/dp is a dimensionless quantity [1]. The linearly interpolated dCij/p values for GaxIn1xPyAs1y/InP are shown in Figure 3.10. The binary data are taken from Table 3.8 in Adachi [1]. Like dCij/dT in Figure 3.8, the dCij/dp versus y plots show very weak nonlinearity with respect to y. 6 5 4 3 2 6

Gax In1-x Py As1-y /InP

(a)

5 4

(b)

dC44 /dp

3 0.8 (c)

0.6 0.4 0.2 0

0.2

0.4

y

0.6

0.8

1.0

Figure 3.10 Linearly interpolated dCij/dp versus y for GaxIn1xPyAs1y/InP at 300 K. The binary dCij/dp values used in the calculation (Equation (A.6)) are taken from Adachi [1]

Maheswaranathan et al. [8] measured the pressure coefficients dCij/dp of CdTe and ZnxCd1xTe for p up to 4 kbar. They obtained dC11/dp ¼ 3.6 0.1, dC12/dp ¼ 4.4 0.1 (296 K) and dC44/dp ¼ 1.99 0.01 (196 K) for CdTe; dC11/dp ¼ 4.0 0.1, dC12/dp ¼ 4.4 0.1 (296 K) and dC44/dp ¼ 2.38 0.02 (196 K) for Zn0.48Cd0.52Te.

ELASTIC PROPERTIES

89

3.2 THIRD-ORDER ELASTIC CONSTANT No experimental data has been reported on the third-order elastic constants (Cijk) of group-IV, III–Vor II–VI semiconductor alloys. This necessitates the use of some sort of an interpolation scheme. The reported Cijk values for some non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Tables 3.11 and 3.12 of Adachi [1].

3.3 YOUNG’S MODULUS, POISSON’S RATIO AND SIMILAR PROPERTIES 3.3.1 Group-IV Semiconductor Alloy The general properties of various elastic moduli, such as Young’s modulus and Poisson’s ratio, are presented in Adachi [1]. The alloy Cij values can be estimated with good accuracy using the linear interpolation scheme (Section 3.1.2). Thus, the various elastic moduli can be calculated from the linearly interpolated Cij values. The expressions of the various elastic moduli can be found in Adachi [1]. As an example, the bulk moduli Bu calculated from the linearly interpolated Cij values of CxSi1x (dashed line) are illustrated in Figure 3.11. The endpoint and 3C-SiC data are shown by the open and solid circles, respectively [1]. These data show weak downward bowing (solid line). 500

Bu (GPa)

400

CxSi1-x

300 200 3C-SiC

100 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.11 Bulk modulus Bu versus x for CxSi1x at 300 K calculated using the linearly interpolated Cij values (dashed line). The endpoint and 3C-SiC values are shown by the open and solid circles, respectively [1]. These experimental data exhibit weak downward bowing (solid line)

Using a Monte Carlo simulation, Kelires [10] found that CxSi1x exhibits an accurate power-law dependence of Bu on the lattice constant a or, equivalently, on the average nearestneighbor distance d, over the whole composition range.

3.3.2 III–V Semiconductor Alloy A technique using XRD was demonstrated for the simultaneous determination of Poisson’s ratio P, lattice constant a and composition x for some III–V ternaries [11]. In Figure 3.12 P versus x has been plotted for (a) AlxIn1xAs, (b) GaxIn1xP and (c) GaxIn1xAs. The solid lines represent the results calculated from the linearly interpolated Cij values.

90

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.40 P

0.35 0.30

(a) Alx In1-x As

0.25 0.40 P

0.35 0.30

(b) Gax In1-xP

0.25 0.40 P

0.35 0.30 0.25

(c) Gax In1-x As

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.12 Poisson’s ratio P versus x for (a) AlxIn1xAs, (b) GaxIn1xP and (c) GaxIn1xAs at 300 K. The solid lines represent the P versus x curves calculated from the linearly interpolated Cij values. The solid circles show the experimental data taken from Hoke et al. [11], while the open circles represent the endpoint binary data taken from Adachi [1]

Figure 3.13 shows the bulk modulus Bu as a function of y for GaxIn1xPyAs1y/InP. The solid line represents the Bu versus y curve calculated from the linearly interpolated Cij values. The experimental data plotted are taken from Prins and Dunstan [12]. The experimental Bu data are found to be the same as InP to within 1%, while Ga0.47In0.53As (y ¼ 0) is 5% lower. 90 Gax In1-x Py As1-y /InP

Bu (GPa)

80 70 60 50

0

0.2

0.4

y

0.6

0.8

1.0

Figure 3.13 Bulk modulus Bu versus y for GaxIn1xPyAs1y/InP at 300 K. The solid line represents the Bu versus y curve calculated from the linearly interpolated Cij values. The solid circles represent the experimental data taken from Prins and Dunstan [12]. The open circle also represents the InP data taken from Adachi [1]

Caro et al. [13] determined Poisson’s ratio P of AlxGa1xAs using a HRXRD. They concluded that both the lattice parameter a and Poisson’s ratio P are in agreement with Vegard law.

3.3.3 II–VI Semiconductor Alloy The elastic constants Cij for the Be-based II–VI semiconductors, BeS, BeSe and BeTe listed in Table 3.1, are estimated from the simple Cij–a (lattice parameter) relationship in Adachi [1].

ELASTIC PROPERTIES

91

These elastic constants yield the bulk moduli Bu of 90, 81 and 67 GPa for BeS, BeSe and BeTe, respectively. On the other hand, the experimental data were Bu ¼ 92.2 1.8 GPa for BeSe and 66.8 0.7 GPa for BeTe if the pressure derivatives dBu/dp were fixed at 4 [14]. 80

10 c-ZnxCd1-xSe

8 6

Bu

40

4 dBu /dp

20 0

0

0.2

0.4

x

0.6

dBu /dp

Bu (GPa)

60

2 0.8

0 1.0

Figure 3.14 Bulk modulus Bu and pressure derivative dBu/dp versus x for c-ZnxCd1xSe at 300 K. The solid line represents the Bu versus y curve calculated using the linearly interpolated Cij values. The solid line for dBu/dp is also obtained from the linear interpolation scheme using the endpoint binary data in Adachi [1] (open triangles). The experimental data (x ¼ 0.9) are taken from Lin et al. [15]

The WDXS technique was employed to study the elastic properties of ZnxM1xSe (M ¼ Cd, Fe or Mn) [15]. Figure 3.14 shows the ZnxCd1xSe data for x ¼ 0.9. The Bu versus x curve is calculated from the linearly interpolated Cij values, while the dBu/dp curve is simply obtained from the linear interpolation between the endpoint values in Adachi [1]. The pressure derivative of Bu can now be written as [1] dBu 1 dC11 2 dC12 ¼ þ 3 dp 3 dp dp

ð3:2Þ

The bulk moduli Bu of ZnSexTe1x (0 x 1.0) have been determined using the WDXS [16]. These data are presented in Figure 3.15. The solid line shows the linear least-squares fit given by Bu ðxÞ ¼ 53:0 þ 13:5x

ð3:3Þ

80 ZnSexTe1-x

Bu (GPa)

70 60 50 40

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.15 Bulk modulus Bu versus x for ZnSexTe1x at 300 K. The experimental data are taken from Pellicer-Porres et al. [16]. The solid line represents the least-squares fit of Equation (3.3). The open circles show the endpoint binary data taken from Adachi [1]

92

PROPERTIES OF SEMICONDUCTOR ALLOYS

The x-dependent Young’s moduli Y have been determined for BexZn1xSe grown on GaP(100) and GaAs(100) by MBE [17]. The measured Y values increased almost linearly with increasing x. However, these data are slightly larger than the generally accepted values, e.g. about 10% larger for ZnSe.

3.4 MICROHARDNESS 3.4.1 Group-IV Semiconductor Alloy No detailed studies relating to the microhardness of group-IV semiconductor alloys have been found in the literature. The hardness values H for Si, diamond and 3C-SiC are shown graphically in Figure 3.16. The experimental data are taken from Table 3.23 in Adachi [1]. The 3C-SiC value deviates slightly from the weighted average of diamond and Si. 140 120

CxSi1-x

H (GPa)

100 3C-SiC

80 60 40 20 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 3.16 Microhardness H versus x for CxSi1x at 300 K. The endpoint and 3C-SiC values are plotted by the solid circles. These data are taken from Adachi [1]. The solid line represents the linear interpolation result between the endpoint elemental data

3.4.2 III–V Semiconductor Alloy Several authors have carried out measurements on the microhardness H of III–V semiconductor alloys. The H values for some (Al, Ga)- and (Ga, In)-based ternaries are shown in Figures 3.17 and 3.18, respectively. The experimental data in Figure 3.17 are taken from Caceres et al. [18] and Hjort et al. [19] and in Figure 3.18 from Bourhis and Patriarche [20] and Schenk and Silber [21]. The open circles represent the data taken from Adachi [1]. It can be seen from Figures 3.17 and 3.18 that the microhardness is almost linear with respect to x, except in the case of GaxIn1xP. The considerable strengthening observed in GaxIn1xP (x 0.5) was attributed to the high crystal friction as confirmed by the flow-stress values [20]. The microhardness anisotropy was determined for GaxIn1xPyAs1y/InP. Figure 3.19 shows the 3D representation of the Knoop hardness anisotropy on the (100) surfaces of GaxIn1xPyAs1y/InP with y as a parameter [22]. The ternary (y ¼ 0) and quaternary hardness anisotropy in Figure 3.19 share a general shape, which is fundamentally different from that of InP, having two or more maxima and one or more minima instead of one maximum and two minima. The major slip system in the diamond and zinc-blende structures is 1/2 {111}. Dislocations generated by plastic deformation, therefore, lie on the {111} planes with

ELASTIC PROPERTIES 24

93

12

21

10

H (GPa)

18 8

15 12

6

9

4

6 (a) w-AlxGa1-xN

3 0

0

0.2 0.4 0.6 0.8 1.0 x

2 0

(b) AlxGa1-xAs 0

0.2 0.4 0.6 0.8 1.0 x

Figure 3.17 Microhardness H versus x for (a) w-AlxGa1xN and (b) AlxGa1xAs at 300 K. The experimental data in (a) are taken from Caceres et al. [18] and in (b) from Hjort et al. [19]. The solid line in (b) shows the linear interpolation result between the endpoint binary data [1]

18

6 (a) GaxIn1-xP

H (GPa)

15 12

4

9

3

6

2

3

1

0

0

0.2 0.4 0.6 0.8 1.0 x

(b) GaxIn1-xSb

5

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 3.18 Microhardness H versus x for (a) GaxIn1xP and (b) GaxIn1xSb at 300 K. The experimental data in (a) are taken from Bourhis and Patriarche [20] and in (b) from Schenk and Silber [21] (heavy solid line). The solid lines show the linear interpolation results between the endpoint binary data [1]

1/2 Burgers vectors. The radically different shape of the anisotropy curves observed may suggest significant differences between the deformation behavior of the alloys and InP, which might be associated with different dislocation dynamics and even, perhaps, a primary slip system different from the , {111} system. The composition dependence of the average Knoop hardness H in Figure 3.19 shows that H increases with increasing y from the ternary value (5.2 GPa), peaking at y 0.5 (H 5.4 GPa), and decreasing with further increases of y (H 4 GPa at y ¼ 1.0) [22].

3.4.3 II–VI Semiconductor Alloy The microhardness of BeO has been reported to be H 0.92–13 GPa [23]. There has, however, been no experimental data for H in BeS, BeSe and BeTe. Alloying ZnSe with a more covalent II–VI compound such as BeSe may significantly alter the mechanical properties and eventually

94

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 3.19 Three-dimensional representation of microhardness anisotropy observed on (1 0 0)oriented GaxIn1xPyAs1y/InP with y as a parameter (y ¼ 0–1.0) at 300 K. [Reproduced with permission from D. Y. Watts and A. F. W. Willoughby, J. Mater. Sci. 23, 272 (1988), Copyright (1988) Springer]

lead to viable devices. In particular, both hardness and elastic modulus are expected to be enhanced by increasing the bond covalency. The composition dependence of H for BexZn1xSe has been investigated by several authors. We summarize these results in Figure 3.20. The experimental data are taken from Waag et al. [24] (open circles) and Paszkowicz et al. [25] (solid circles). The solid line also shows the experimental data of Grillo et al. [26]. Although there is a large difference in H, all these data show an increase in H with increasing x. The data of Grillo et al. [26] show a peak in H at x 0.7. 10 Bex Zn1-x Se

H (GPa)

8 6 4 2 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 3.20 Microhardness H versus x for BexZn1xSe at 300 K. The experimental data are taken from Waag et al. [24] (open circles) and Paszkowicz et al. [25] (solid circles). The solid line also represents the experimental data by Grillo et al. [26]

The microhardness H for ZnSexTe1x (0 x 0.06) and BexZn1xSeyTe1y (0 x 0.11) has been measured by Maruyama et al. [27]. These data show an increase in H with increasing Se or Be concentration. Figure 3.21 shows the experimental H data for ZnxHg1xSe as measured by Fang et al. [28]. The open circles represent the endpoint data taken from Adachi [1]. The solid line represents the linearly interpolated result. The experimental curve shows a pronounced peak at

ELASTIC PROPERTIES

95

Figure 3.21 Microhardness H versus x for ZnxHg1xSe at 300 K. [Reproduced with permission from S. Fang, L. J. Farthing, M.-F. S. Tang, and D. A. Stevenson, J. Vac. Sci. Technol. A 8, 1120 (1990). Copyright (1990), American Vacuum Society]. The solid line shows the linear interpolation result between the endpoint binary data [1]

x 0.7. Similarly, the experimental curve for ZnxCd1xTe obtained by Schenk and Dunog [29] showed a peak at x 0.7, as shown in Figure 3.22. A peak at x 0.7 was also observed in CdxHg1xTe [28]. The microhardness at x 0.7 in ZnxHg1xSe is about 1.6 GPa, which is at least twice the value of that in CdxHg1xTe. The microhardness H of CdxHg1xTe decreased with increasing temperature from 300 to 600 K, e.g. from H 0.7 GPa at 300 K to 0.2 GPa at 600 K for x ¼ 0.7 [30].

Figure 3.22 Microhardness H versus x for ZnxCd1xTe at 300 K. [Reproduced with permission from M. Schenk and L. T. H. Dunog, Semicond. Sci. Technol. 13, 335 (1998), Copyright (1998) Institute of Physics]. The solid line shows the linear interpolation result between the endpoint binary data [1]

Generally, isoelectronic doping in the order of ppm leads to a softening of the crystal lattice due to the vacancies in the lattice being filled with dopant atoms, and hence the etch-pit density is reduced, virtually without affecting the electrical properties of the material. Softening as a result of isoelectronic doping has been observed in In-doped GaAs [31] and in Zn-doped CdS [32].

96

PROPERTIES OF SEMICONDUCTOR ALLOYS

In conclusion of this section, the microhardness H of some tetrahedral semiconductor alloys shows a liner relationship between H and the alloy composition. More ionic semiconductor alloys, namely, II–VI alloys, however, show not only a clear upward bowing, but also a deviation from the parabolic behavior of the microhardness H. Such deviations lead to a peak in H at x 0.7 and not at x 0.5.

3.5 SOUND VELOCITY If the crystal density g and elastic stiffness Cij of a solid are known, the sound velocity v can be calculated from the simple relationship sﬃﬃﬃﬃﬃﬃ Cij v¼ g

ð3:4Þ

The detailed functional forms, in terms of Cij, of Equation (3.4) are shown in Tables 3.25 and 3.27 of Adachi [1]. The alloy Cij and g values can be approximated with good accuracy by the linear interpolation scheme. Thus, we can easily calculate the sound velocities propagating in the various crystallographic directions. For example, Figure 3.23 shows the calculated sound velocities propagating in the [110] direction in (a) AlxGa1xAs and (b) GaxIn1xPyAs1y/InP, where vLA corresponds to the longitudinal mode and vTA1 and vTA2 correspond to the slow and fast transverse modes, respectively. It can be seen that the sound velocities propagating in these alloys exhibit a weak nonlinear dependence on x or y.

7 6

7 6

vLA

v (105 cm/s)

5

(b) Gax In1-x PyAs1-y /InP vLA

5

4

4

vTA2

3

vTA2

3 vTA1

2 1 0 0

2 1

(a) AlxGa1-x As 0.2

0.4

0.6 x

vTA1

0.8

1.0

0 0

0.2

0.4

0.6

0.8

1.0

y

Figure 3.23 Sound velocities propagating in the [1 1 0] direction in (a) AlxGa1xAs and (b) GaxIn1x PyAs1y/InP, where vLA corresponds to the longitudinal mode and vTA1 and vTA2 correspond to the slow and fast transverse modes, respectively

ELASTIC PROPERTIES

97

Note that in piezoelectric semiconductors like GaAs and GaN, the sound velocity given by Equation (3.4) should be modified as sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Cij þ K 2 v¼ g

ð3:5Þ

where K2 is the electromechanical coupling constant [1], which leads to a piezoelectrically stiffened elastic constant if the sound wave is involved with piezoelectricity. The change in sound velocity due to piezoelectricity is only 0.1% for GaAs, but is 0.5% for GaN [33].

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] M. Mendik, M. Ospelt, H. von K€anel, and P. Wachter, Appl. Surf. Sci. 50, 303 (1991). [3] G. Galibert and G. Bougnot, Mater. Res. Bull. 9, 167 (1974). [4] G. Carlotti, D. Fioretto, L. Palmieri, G. Socino, A. Verdini, and C. Rigo, J. Phys.: Condens. Matter 8, 2265 (1996). [5] A. Hassine, J. Sapriel, P. L. Berre, P. Legay, F. Alexandre, and G. Post, J. Appl. Phys. 77, 6569 (1995). [6] F. C. Peiris, U. Bindley, J. K. Furdyna, H. Kim, A. K. Ramdas, and M. Grimsditch, Appl. Phys. Lett. 79, 473 (2001). [7] I. I. Andrusiv, G. M. Grigorovich, Y. V. Ilisavskiıˇ, M. A. Ruvinskiıˇ, and V. P. Shchetinin, Sov. Phys. Solid State 25, 139 (1983). [8] P. Maheswaranathan, R. J. Sladek, and U. Debska, Phys. Rev. B 31, 5212 (1985). [9] D. T. Queheillalt and H. N. G. Wadley, J. Appl. Phys. 83, 4124 (1998). [10] P. C. Kelires, Phys. Rev. B 55, 8784 (1997). [11] W. E. Hoke, T. D. Kennedy, and A. Torabi, Appl. Phys. Lett. 79, 4160 (2001). [12] A. D. Prins and D. J. Dunstan, Semicond. Sci. Technol. 4, 239 (1989). [13] L. D. Caro, C. Giannini, L. Tapfer, H.-P. Sch€onherr, L. D€aweritz, and K. H. Ploog, Solid State Commun. 108, 77 (1998). [14] H. Luo, K. Ghandehari, R. G. Greene, and A. L. Ruoff, Phys. Rev. B 52, 7058 (1995). [15] C.-M. Lin, D.-S. Chuu, J. Xu, E. Huang, W.-C. Chou, J.-Z. Hu, and J.-H. Pei, Phys. Rev. B 58, 16 (1998). [16] J. Pellicer-Porres, D. Martinez-Garcia, C. Ferrer-Roca, A. Segura, V. Mun˜oz-Sanjose, J. P. Itie, A. Polian, and P. Munsch, Phys. Rev. B 71, 035210 (2005). [17] S. E. Grillo, M. Ducarroir, M. Nadal, E. Tournie, and J.-P. Faurie, J. Phys. D: Appl. Phys. 35, 3015 (2002). [18] D. Caceres, I. Vergara, R. Gonzalez, E. Monroy, F. Calle, E. Mun˜oz, and F. Omnees, J. Appl. Phys. 86, 6773 (1999). [19] K. Hjort, F. Ericson, J.-A. Schweitz, C. Hallin, and E. Janzen, Thin Solid Films 250, 157 (1994). [20] E. L. Bourhis and G. Patriarche, Philos. Mag. Lett. 84, 373 (2004). [21] M. Schenk and C. Silber, J. Mater. Sci.: Mater. Electron. 9, 313 (1998). [22] D. Y. Watts and A. F. W. Willoughby, J. Mater. Sci. 23, 272 (1988). [23] L. Garrato and A. Rucci, Philos. Mag. 35, 1681 (1977). [24] A. Waag, F. Fischer, H.-J. Lugauer, T. Litz, T. Gerhard, J. N€ urnberger, U. Lunz, U. Zehnder, W. Ossau, G. Landwehr, B. Roos, and H. Richter, Mater. Sci. Eng. B 43, 65 (1997).

98

PROPERTIES OF SEMICONDUCTOR ALLOYS

[25] W. Paszkowicz, K. Godwod, J. Domagała, F. Firszt, J. Szatkowski, H. Me˛czy nska, S. Łe˛gowski, and M. Marczak, Solid State Commun. 107, 735 (1998). [26] S. E. Grillo, M. Ducarroir, M. Nadal, E. Tournie, and J.-P. Faurie, J. Phys. D: Appl. Phys. 35, 3015 (2002). [27] K. Maruyama, K. Suto, and J. Nishizawa, Jpn. J. Appl. Phys. 39, 5180 (2000). [28] S. Fang, L. J. Farthing, M.-F. S. Tang, and D. A. Stevenson, J. Vac. Sci. Technol. A 8, 1120 (1990). [29] M. Schenk and L. T. H. Dunog, Semicond. Sci. Technol. 13, 335 (1998). [30] J. F. Barbot, G. Rivaud, H. Garem, C. Blanchard, J. C. Desoyer, D. Le-Scoul, J. L. Dessus, and A. Durand, J. Mater. Sci. 25, 1877 (1990). [31] S. Kouba€ıti, C. Levade, J. J. Couderc, and G. Vanderschaeve, Eur. Phys. J. Appl. Phys. 1, 141 (1998). [32] K. Balakrishnan, J. Kumar, and P. Ramasamy, J. Mater. Sci. Lett. 14, 720 (1995). [33] C. Deger, E. Born, H. Angerer, O. Ambacher, M. Stutzmann, J. Hornsteiner, E. Riha, and G. Fischerauer, Appl. Phys. Lett. 72, 2400 (1998).

4 Lattice Dynamic Properties 4.1 PHONON DISPERSION RELATIONSHIPS Theoretical work on the lattice dynamics of semiconductor alloys has been carried out by several authors. For example, Myles [1] evaluated the spectral density of phonon states for 1D mass-disordered alloys using a generalized embedded-cluster method. Baroni et al. [2] studied the lattice vibronic properties of AlxGa1xAs using large supercells to simulate the disorder and ab initio interatomic force constants. They found that there are well-defined AlAs- and GaAslike phonon dispersions for any concentration, in agreement with experimental evidence [3]. In addition to broadening phonon states with definite wavevectors, alloying also narrows the optical phonon branches and lowers the longitudinal modes more than the transverse modes, thus reducing the LO–TO splitting. The acoustic phonon bands are in contrast also found to be rather insensitive to the alloy composition.

4.2 PHONON FREQUENCY 4.2.1 General Considerations Lattice vibronic properties in semiconductor alloys have received a great deal of attention over a long period of time [4]. The defect-induced local or gap modes for small concentrations of impurities are broadened into vibrational bands for high impurity concentrations as in solid solutions. In an AxB1xC alloy, such vibrational bands exhibit either one-mode or twomode behavior (or more rigorously, three different types of mode behavior, namely, one-, two- and one-two-mode (mixed-mode) behaviors; see Figure 4.1). In a one-mode system (Figure 4.1(a)), such as most I–VII alloys, a single set of long-wavelength optical phonons appear. The one-mode phonon spectrum is approximately constant in strength but varies in energy as the alloy composition is varied from one end member to another. The two-mode system (Figure 4.1(b)), which is common for III–V ternaries, exhibits two distinct sets of optical modes with frequencies characteristic of each end member and strengths roughly proportional to the respective concentration. The one-two-mode system exhibits a single mode over only a part of the composition range, with two modes observed over the remaining range of composition (Figures 4.1(c) and 4.1(d)). A number of models have been proposed to explain the so-called multi-mode behavior in solid solutions [5]. Of these different models, the MREI model of Chang and Mitra [5,6] appears to be the most successful. In the MREI model, if an alloy AxB1xC has the relationship MA < mBC Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

ð4:1Þ Sadao Adachi

100

PROPERTIES OF SEMICONDUCTOR ALLOYS

LO 1

LO 1

LO 1

LO

ω LO, TO

TO 1

TO 1

LO 2

TO 1 LO 2

LO 2

TO TO 2

TO2

TO 2

Local mode Gap mode

(a) 0

0.5 x

1.0 0

(b) 0.5 x

1.0 0

(c) 0.5 x

1.0 0

(d) 0.5 x

1.0

Figure 4.1 Four different types of long-wavelength phonon mode behavior in ternary alloy: (a) onemode; (b) two-mode; (c) one-two-mode (1); (d) one-two-mode (2) 1 1 it exhibits two-mode behavior. Here,m1 BC ¼ MB þ MC is the reduced mass of the binary material BC. The opposite is true for one-mode behavior. In other words, for an alloy to exhibit two-mode (one-mode) behavior it must (must not) have one substituting element whose mass is smaller than the reduced mass of the compound formed by the other two elements. Given the masses of the end members, the MREI model can predict whether an alloy will show one- or two-mode behavior and also the dependence of the optical phonon frequencies on x [5, 6]. Table 4.1 summarizes the long-wavelength optical phonon frequencies, h¯ vLO and h¯ vTO, for a number of cubic group-IV, III–Vand II–VI semiconductors at 300 K and Table 4.2 lists those for some hexagonal III–V and II–VI semiconductors at 300 K. In an ordered alloy Ga0.5In0.5P, four additional phonon modes at 60, 205, 310 and 354 cm1, attributed to spontaneous ordering in this material, have been identified and explained using various experimental techniques [7]. However, a major obstacle to further enhancing the understanding of this subject is the lack of a theoretical model that can satisfactorily explain the experimental optical phonon frequencies and selection rules in ordered alloys. In the following, the data mainly refers to fully disordered semiconductor alloys.

4.2.2 Room-temperature Value (a) Group-IV semiconductor alloy The experimental long-wavelength optical phonon frequencies vLO and vTO for 3C-SiC, together with those for diamond and Si, are shown in Figure 4.2. 3 C-SiC is considered to be an ordered alloy, or more succinctly, it is a compound, not an alloy. Note that for diamond-type structures the LO and TO branches are degenerate at q ¼ 0 and thus vLO ¼ vTO. The solid line in Figure 4.2 shows the linear interpolation result between Si (x ¼ 0) and diamond (x ¼ 1.0). The 3C-SiC values can be satisfactorily interpreted by the average values of Si and diamond. SixGe1x has three types of cell and consequently shows multi-mode behavior consisting of three main peaks due to the vibrations of SiSi, GeGe and SiGe pairs (Table 4.3). The composition dependence of the SiSi, SiGe and GeGe mode frequencies for SixGe1x

LATTICE DYNAMIC PROPERTIES

101

Table 4.1 Long-wavelength optical phonon frequencies, h¯ vLO and h¯ vTO, for some cubic group-IV, IIIV and IIVI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt h¯ vLO (cm1)

h¯ vTO (cm1)

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

1332 519.2 301 200 972

1332 519.2 301 200 796

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

1305 828.9 902 501.0 402 340.0 739 402.5 292 233 586 346.4 241.4 190.7

1054.7 799 655 439.4 362 318.7 553 365.3 268 224 455 304.5 219.6 179.7

II–VI

BeSe (zb) BeTe (zb) MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

576 502 725 425 340 292 350.5 252 210 478 303a 211a 167 224 174 135

496 461 401 327 237 235 272.0 205 181 262 237a 169a 139 177 132 116

System

Material

IV

a

Calculated or estimated

is shown in Figure 4.3(a). The experimental data were obtained from Pezzoli et al. [8]. The homopolar-bond frequencies vary almost linearly with x, while the heteropolar-bond frequency shows a maximum at x 0.5. These can be written as (in cm1) vSiSi ðxÞ ¼ 52167x

ð4:2aÞ

102

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 4.2 Long-wavelength optical phonon frequencies for some hexagonal III–V and II–VI semiconductors at 300 K. h ¼ hexagonal (P63/mmc (D6h)); w ¼ wurtzite System

Phonon frequency (cm1)

Material E2 low

A1 (TO)

E1 (TO)

E2 high

A1 (LO)

E1 (LO)

III–V

BN (h) AlN (w) GaN (w) InN (w)

49 248 144 87

770 610 533 457

1383 670 560 490

1367 657 569 475

778 890 736 588

1610 915 743 582

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

340 100 65 41 34

680 380 270 233 166

724 410 273 239 170

684 439 281 255

1083 576 350 301 210

1098 587 350 304 211

Cx Si1-x

3C-SiC

ω LO, TO (cm-1)

1500 1200

ω LO

900

ω TO

600 300

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.2 Long-wavelength optical phonon frequencies vLO and vTO for 3C-SiC at 300 K, together with those for diamond and Si. The solid line represents the linear interpolation result between the endpoint elemental data

Table 4.3 Long-wavelength optical phonon mode observed in some group-IV semiconductor alloys Alloy

Phonon mode

Reference

SiGe CSiGe SiGeSn

SiSi, GeGe, SiGe SiSi, GeGe, CSi, CGe (?), SiGe SiSi, GeGe, SiGe, SnSn

a b c

F. Pezzoli et al., Mater. Sci. Eng. B 124–125, 127 (2005) C 0.3 at% (M. Melendez-Lira et al., Phys. Rev. B 54, 12866 (1996)) c Si 20 at%, Sn 10 at% (V. R. DCosta et al., Phys. Rev. B 76, 035211 (2007)) a b

LATTICE DYNAMIC PROPERTIES

103

Figure 4.3 (a) Three main optical phonon frequencies due to the vibrations of SiSi, SiGe and GeGe pairs versus x for SixGe1x at 300 K. (b) Relative Raman intensities against x for SixGe1x at 300 K. [Reprinted with permission from Mater. Sci. Eng. B, Raman spectroscopy of Si1xGex epilayers by F. Pezzoli et al., 124–125, 127. Copyright (2005), Elsevier]

vGeGe ðxÞ ¼ 280 þ 19x

ð4:2bÞ

for the homopolar-bond modes and vSiGe ðxÞ ¼ 400 þ 24:5x4:5x2 33:5x3

ð4:3Þ

for the heteropolar-bond mode. The corresponding Raman intensities are plotted in Figure 4.3(b). The probability of finding SiSi, SiGe and GeGe vibrating pairs is proportional to the relative numbers of the bond types: x2, 2x(1 x) and (1 x)2, respectively. The experimental data in Figure 4.3(b) follow this statistic very well. The ordering effect and/or compositional fluctuation should influence the vibronic properties of alloys, and in particular, the relative intensities and linewidths of the Raman modes. Tsang et al. [9] measured the Raman spectra of compositionally ordered Si0.5Ge0.5 layers and compared them to the spectrum of a random alloy. They observed changes in the relative intensities of the different optical phonons, suggesting that the ordering is associated with an increase in the number of homopolar bonds and a decrease in the number of heteropolar bonds. The Raman scattering data also suggested that the ordering is not complete; the changes in the Raman intensities are quantitatively consistent with XRD-estimated ordering of 80%. The effects of substitutional carbon in SixGe1x have been studied by several authors [10–12]. Because of the significant difference in covalent bond radii between Si and C atoms, the C defect in the Si lattice is surrounded by a considerable strain field, with substitutional defect bonds under tensile strain and interstitial bonds under compressive strain. A substitutional C defect in SixGe1x is expected to be surrounded by an even stronger strain field than

104

PROPERTIES OF SEMICONDUCTOR ALLOYS

that in pure Si, due to the increase in the C bond lengths with the Ge atoms. Interstitial C defects will be under smaller compressive strain due to the increase in the average lattice constant with Ge. The experimental frequencies of the SiSi, GeGe and SiGe modes in SixGe1x increased as a function of C concentration, which can be explained qualitatively in terms of the large bond distortions caused by the lattice mismatch between SixGe1x and diamond [10]. A number of phonon modes associated with the substitutional C defects in SixGe1x have been detected and attributed to localized phonon modes of C defects with different nearest-neighbor configurations of Si and Ge atoms (Table 4.3). (b) III–V semiconductor alloy Most IIIV ternaries exhibit two-mode behavior. Some IIIV ternaries exhibit one- or onetwo-mode behavior. These are summarized in Table 4.4. The long-wavelength optical phonon Table 4.4 Behavior of the long-wavelength optical phonon modes in some III–V semiconductor alloys. zb ¼ zinc-blende; w ¼ wurtzite; O ¼ one mode; T ¼ two mode; O-T ¼one-two mode; Tr-F ¼ three-four mode; Tr ¼ three mode; F ¼ four mode; T-Tr ¼ two-three mode Alloy

Material

Behavior

Reference

Ternary

AlGaN (zb) AlGaN (w) AlInN (w) AlGaP (zb) AlGaAs (zb) AlGaSb (zb) AlInP (zb) AlInAs (zb) AlInSb (zb) GaInN (zb) GaInN (w) GaInP (zb) GaInAs (zb) GaInSb (zb) AlAsSb (zb) GaNP (zb) GaNAs (zb) GaPAs (zb) GaPSb (zb) GaAsSb (zb) InPAs (zb) InPSb (zb) InAsSb (zb)

O (LO), T (TO) T (E1(TO)), O (others) O (A1(LO), E1(LO)), T (others) O O (E1(TO)) T T T T T T O O T T O-T O T T T T T T T O-T

a b c d e f g h i j k l m n o p q r s t u v w x y

AlGaPAs (zb) AlGaAsSb (zb) GaInPSb (zb)

Tr-F Tr F

z aa ab

Quaternary

(continued)

LATTICE DYNAMIC PROPERTIES

105

Table 4.4 (Continued) Alloy

Material

Behavior

Reference

GaInPAs/InP (zb) GaInPAs/GaAs (zb) GaInAsSb (zb) AlGaInP/GaAs (zb) AlGaInAs/InP (zb) InPAsSb (zb)

F F Tr T-Tr Tr Tr

ac ad ae af ag ah

H. Harima et al., Appl. Phys. Lett. 74, 191 (1999) M. Kazan et al., J. Appl. Phys., 100, 013508 (2006) c V. Y. Davydov et al., Phys. Rev. B 65, 125203 (2002) d M. S. Liu et al., J. Appl. Phys. 90, 1761 (2001) e A. Kasic et al., Appl Phy. Lett. 78, 1526 (2001) f G. Armelles et al., Solid State Commun. 65, 779 (1988) g D. J. Lockwood and Z. R. Wasilewski, Phys. Rev. B 70, 155202 (2004) h R. Ferrini et al., Phys. Rev. B 56, 7549 (1997) i H. Asahi et al., J. Appl. Phys. 65, 5007 (1989) j S. Emura et al., J. Appl. Phys. 62, 4632 (1987) k V. P. Gnezdilov et al., J. Appl. Phys. 74, 6883 (1993) l K. Torii et al., Appl. Phys. Lett. 82, 52 (2003) m S. Hernandez et al., J. Appl. Phys. 98, 013511 (2005) n B. Jusserand and S. Slempkes, Solid State Commun. 49, 95 (1984) o Z. S. Piao et al., Phys. Rev. B 50, 18644 (1994) p Z. C. Feng et al., Can. J. Phys. 69, 386 (1991) q H. C. Lin et al., Solid State Commun. 107, 547 (1998) r G. Leibiger et al., Appl. Phys. Lett. 79, 3407 (2001) s T. Prokofyeva et al., Appl. Phys. Lett. 73, 1409 (1998) t G. Armelles et al., Appl. Phys. Lett. 68, 1805 (1996) u Y. T. Cherng et al., J. Appl. Phys. 65, 3285 (1989) v T. C.McGlinn et al., Phys. Rev. B 33, 8396 (1986) w D. J. Lockwood et al., J. Appl. Phys. 102, 033512 (2007) x M. J. Jou et al., J. Appl. Phys. 64, 1472 (1988) y N. L. Rowell et al., J. Vac. Sci. Technol. A 22, 935 (2004) z P. N. Sen and G. Lucovsky, Phys. Rev. B 12, 2998 (1975) aa D. H. Jaw et al., J. Appl. Phys. 69, 2552 (1991) ab D. H. Jaw and G. B. Stringfellow, J. Appl. Phys. 72, 4265 (1992) ac T. Sugiura et al., Jpn. J. Appl. Phys. 37, 544 (1998) ad T. Sugiura et al., Jpn. J. Appl. Phys. 32, 2718 (1993) ae D. H. Jaw et al., J. Appl. Phys. 66, 1965 (1989) af T. Hofmann et al., Phys. Rev. B 64, 155206 (2001) ag R. Manor et al., Phys. Rev. B 56, 3567 (1997) ah L.-C. Chen et al., Jpn. J. Appl. Phys. 37, L1365 (1998) a b

frequencies vLO and vTO versus x for (a) c-AlxGa1xN and (b) c-GaxIn1xN are shown in Figure 4.4. The experimental data for c-AlxGa1xN are taken from Harima et al. [13] and for c-GaxIn1xN from Tabata et al. [14] and Torii et al. [15]. The LO phonon frequencies in Figure 4.4(a) exhibit one-mode behavior, while the twomode behavior is observed for the TO phonon frequencies. The mass criterion of Equation (4.1) suggests that AlxGa1xN may exhibit one-mode behavior (MAl,Ga > mAlN,GaN). Harima

106

PROPERTIES OF SEMICONDUCTOR ALLOYS 1000

800

(a)

ω LO, TO (cm-1)

900

(b) c-Gax In1-x N

c-AlxGa1-x N

800

700 LO

LO

600 700 TO TO (AlN)

600

500

TO (GaN)

500

0

0.2

0.4

0.6

0.8

1.0

400

0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 4.4 Long-wavelength optical phonon frequencies vLO and vTO versus x for (a) c-AlxGa1xN and (b) c-GaxIn1xN at 300 K. The experimental data for c-AlxGa1xN are taken from Harima et al. [13] and for c-GaxIn1xN from Tabata et al. [14] and Torii et al. [15]. The solid line in (a) shows the linear interpolation result between the endpoint binary data (LO). The solid lines in (b) represent the linear interpolation results of Equation (4.4)

et al. [13] calculated the phonon frequencies using the MREI model and considered that the two-mode behavior of vTO is a consequence of the different vibrating masses. In Figure 4.4(b), clear one-mode phonon behavior of c-GaxIn1xN can be seen, in agreement with the criterion of Equation (4.1) (MGa,In > mGaN,InN). The solid lines represent the linear interpolation results (in cm1) vLO ðxÞ ¼ 739153x

ð4:4aÞ

vTO ðxÞ ¼ 55398x

ð4:4bÞ

Figure 4.5 shows the LO and TO phonon frequencies as a function of x for AlxGa1xAs. The experimental data are taken from Jusserand [16]. Only the AlAs-like LO mode exhibits weak nonlinearity with respect to x. Each phonon frequency can be expressed as (in cm1) vLO;AlAs ðxÞ ¼ 354 þ 81x33x2

ð4:5aÞ

vTO;AlAs ðxÞ ¼ 354 þ 8x

ð4:5bÞ

vLO;GaAs ðxÞ ¼ 29237x

ð4:6aÞ

vTO;GaAs ðxÞ ¼ 26813x

ð4:6bÞ

The two-mode behavior in AlxGa1xAs is the most prominent disorder-induced effect (MAl < mGaAs). Additional disorder-induced effects in AlxGa1xAs have been observed, i.e. an asymmetric line broadening and an activation of new phonon bands [16]. A low energy GaAslike LO tail developed when the concentration of Al increased, and vice versa. When this concentration becomes very large, an additional line appears on the lower energy side. Apart from this broadening, additional phonon bands are observed in the TA (100 cm1) and LA

LATTICE DYNAMIC PROPERTIES

107

400

ω LO, TO (cm-1)

LO (AlAs)

350

TO (AlAs)

AlxGa1-xAs 300 LO (GaAs)

250

TO (GaAs)

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.5 Long-wavelength optical phonon frequencies vLO and vTO versus x for AlxGa1xAs at 300 K. The open squares represent the endpoint binary data. The solid lines show the results calculated using Equations (4.5) and (4.6)

range (200 cm1). The asymmetric broadening and the emergence of additional phonon bands can be explained by a disorder activated relaxation of the q ¼ 0 wavevector selection rule. The LO and TO phonon frequencies for GaxIn1xSb determined by Raman scattering at 80 K by Feng et al. [17] are shown in Figure 4.6. They also reported the room-temperature data, which are essentially the same as those at 80 K. In Figure 4.6, the so-called one-two-mode behavior is observed; however, the mass criterion of Equation (4.1) indicates that the alloy will exhibit one-mode behavior (MGa,In > mGaSb,InSb). The one-two-mode behavior was also confirmed using IR spectroscopy [18].

ω LO, TO (cm-1)

250 LO (GaSb)

225

TO (GaSb) 200

LO (InSb) TO (InSb)

175

Gax In1-x Sb

T= 80 K 150

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.6 Long-wavelength optical phonon frequencies vLO and vTO versus x for GaxIn1xSb at 80 K. [Reproduced with permission from Z. C. Feng, S. Perkowitz, R. Rousina, and J. B. Webb, Can. J. Phys. 69, 386–389 (1991), Copyright (1991) NRC Research Press]

108

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.7 Long-wavelength optical phonon frequencies vLO and vTO versus y for GaxIn1xPyAs1y/ InP at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Raman scattering study of InGaAsP quaternary alloys grown on InP in the immiscible region by T. Sugiura et al., 37, 544. Copyright (1998) Japanese Society of Pure and Applied Physics] The open circles represent the InP data

The long-wavelength optical phonon behaviors in GaxIn1xPyAs1y/InP have been studied by Raman and IR spectroscopy [19]. In Figure 4.7 the vLO and vTO frequencies versus y for GaxIn1xPyAs1y/InP are illustrated graphically. The experimental data are taken from Sugiura et al. [20]. The data fall into four separate bands, that is, a four-mode category, except for the GaAs mode at y > 0.6. The composition dependence of vLO and vTO for (AlxGa1x)0.48In0.52As/InP is shown in Figure 4.8. The experimental data were obtained by Raman scattering [21]. Three modes, AlAs-, GaAs- and InAs-like modes, dominate the Raman spectra in (AlxGa1x)0.48In0.52As/ InP. The GaAs- and InAs-like modes vary almost linearly with x. The AlAs-like TO mode also varies linearly with x, but its LO branch exhibits weak nonlinearity with respect to x. The one-mode behavior of AlAsxSb1x and two-mode behavior of GaPxAs1x, GaPxSb1x and InPxAs1x in Table 4.4 agree with the mass criterion of Equation (4.1); however, the twomode behavior observed in GaxIn1xP and GaAsxSb1x is contrary to this criterion. Let us consider GaPxAs1x and GaxIn1xP, the former shows two-mode behavior, while the latter shows one-mode (or a very weak two-mode) behavior. These behaviors are easily understood by noting that the optical-phonon DOS of GaP and GaAs do not overlap unlike those of GaP and InP which do overlap (but in a narrow frequency range). Thus, the two-mode behavior of GaPxAs1x is expected from Equation (4.1) (MP < mGaAs). Because MGa > mGaP,InP, the MREI model predicts one-mode behavior in GaxIn1xP.

LATTICE DYNAMIC PROPERTIES

109

Figure 4.8 Long-wavelength optical phonon frequencies vLO and vTO versus x for (AlxGa1x)0.48 In0.52As/InP at 300 K. [Reproduced with permission from R. Manor, O. Brafman, and R. F. Kopf, Phys. Rev. B 56, 3567–3570 (1997). Copyright (1997) American Physical Society]

(c) II–VI semiconductor alloy II–VI ternaries grow either in the zinc-blende or wurtzite structure and mostly exhibit one- or two-mode behavior, as summarized in Table 4.5. Some II–VI ternaries exhibit a variation with composition that is intermediate between one- and two-mode. Figure 4.9 shows the long-wavelength optical phonon frequencies vLO and vTO as a function of x for ZnxCd1xS. The experimental data are taken from Lucovsky et al. [22]. Since ZnxCd1xS crystallizes in the wurtzite structure, the experimental data produced by Lucovsky et al. shows a small anisotropy splitting (6 cm1) between A1 (LO, TO) and E1 (LO, TO) modes for all values of x. For clarity, however, the averaged vLO and vTO values have been plotted in Figure 4.9. ZnxCd1xS serves a typical example of the one-mode phonon behavior. Figure 4.10 shows the LO and TO phonon frequencies for CdxHg1xTe measured by IR spectroscopy at 77 K [23]. Like ZnxHg1xTe [24], CdxHg1xTe exhibits two-mode behavior. However, the ZnTe-like TO frequency in ZnxHg1xTe increased with increasing Zn content, while the CdTe-like TO phonon mode in CdxHg1xTe (Figure 4.10) decreased with increasing Cd content. This could be due to the fact that the ZnxHg1xTe lattice constant decreases with increasing Zn content but the CdxHg1xTe lattice constant increases with increasing Cd content. Note that the MREI model predicts ZnxHg1xTe to be of the two-mode type (MZn < mHgTe) and CdxHg1xTe to be of the one-mode type (MCd,Hg > mCdTe,HgTe). Both ZnxCd1xSe and ZnSexTe1x exhibit an intermediate-mode behavior [25,26]. As an example, the data for ZnSexTe1x is shown in Figure 4.11 [25]. Not only are the one-mode LO and TO phonons (LO1 and TO1) but also a new LO2–TO2 pair inside the reststrahlen band.

110

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 4.5 Behavior of the long-wavelength optical phonon modes in some II–VI semiconductor alloys. zb ¼ zinc-blende; w ¼ wurtzite; O ¼ one mode; T ¼ two mode; I ¼ intermediate mode; Tr ¼ three mode Alloy

Material

Behavior

Reference

Ternary

BeZnSe BeZnTe MgZnO (zb) MgZnO (w) MgZnO (w) MgZnS MgZnSe MgZnTe MgCdTe ZnCdS ZnCdSe ZnCdTe ZnHgTe CdHgTe ZnSSe ZnSTe ZnSeTe CdSSe CdSTe CdSeTe

Tr Tr T O T (E1), O (A1) O T T T O I T T T T T I T T T

a b c d e f g h i j k l m n o p q o r s

Quaternary

MgZnSSe MgZnSeTe MgZnCdTe ZnCdHgTe CdSSeTe

Tr T Tr Tr Tr

f t h u v

Showing extra BeSe-like mode (O. Pages et al., Phys. Rev. B 70, 155319 (2004)) Showing extra BeTe-like mode (O. Pages et al., Appl. Phys. Lett. 80, 3081 (2002)) c J. Chen and W. Z. Shen, Appl. Phys. Lett. 83, 2154 (2003) d 0 x < 0.3 (Z. P. Wei et al., Phys. Status Solidi C 3, 1168 (2006)) e x0.47–0.60 (J.Chen and W. Z. Shen, Appl. Phys. Lett. 83, 2154 (2003)) f D. Wang et al., J. Appl. Phys. 80, 1248 (1996) g D. Huang et al., Appl. Phys. Lett. 67, 3611 (1995) h R. Vogelgesang et al., J. Raman Spectrosc. 27, 239 (1996) i E. Oh et al., Phys. Rev. B 48, 15040 (1993) j M. Ichimura et al., Phys. Rev. B 46, 4273 (1992) k R. G. Alonso et al., Phys. Rev. B 40, 3720 (1989) l D. N. Talwar et al., Phys. Rev. B 48, 17064 (1993) m M. P. Volz et al., Solid State Commun. 75, 943 (1990) n S. P. Kozyrev et al., Sov. Phys. Solid State 34, 1984 (1992) o I. F. Chang and S. S. Mitra, Phys. Rev. 172, 924 (1968) p Y.-M. Yu et al., J. Appl. Phys. 95, 4894 (2004) q T. R. Yang and C. C. Lu, Physica B 284–288, 1187 (2000) r R. Pal et al., J. Phys. D: Appl. Phys. 26, 704 (1993) s Z. C. Feng et al., J. Cryst. Growth 138, 239 (1994) t H. Makino et al., J. cryst. Growth 214/215, 359 (2000) u J. Polit et al., Phys. Status Solidi B 208, 21 (1998) v V. M. Burlakov et al., Phys. Status Solidi B 128, 389 (1985) a b

LATTICE DYNAMIC PROPERTIES

111

ω LO, TO (cm-1)

400 ZnxCd1-xS

350

ω LO

300 ω TO

250 200

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.9 Long-wavelength optical phonon frequencies vLO and vTO versus x for ZnxCd1xS at 300 K. The experimental data are taken from Lucovsky et al. [22]. The solid lines show the linearly interpolated results between the endpoint binary data

Figure 4.10 Long-wavelength optical phonon frequencies vLO and vTO versus x for CdxHg1xTe at 77 K. [Reprinted with permission from J. Baars and F. Sorger, Solid State Commun. 10, 875 (1972), Copyright (1972) Elsevier]

Pages et al. [27, 28] investigated the Raman spectra of BexZn1xSe and BexZn1xTe. The TO modes were of particular interest because they consist of quasi-independent oscillators and thereby carry clear information. In the LO symmetry, complexity arose due to coupling via the macroscopic polarization field. They observed the atypical TO one-bond ! two-mode behavior in the vibrational range of the stiff Be–VI bond in BexZn1xSe and BexZn1xTe. This was explained by using a double-branch percolation picture which discriminates between vibrations within the randomly formed hard Be-rich host region and the soft Zn-rich region. The resulting phonon frequency versus composition plots showed that the (Be, Zn)–VI ternaries exhibit a three-mode (two usual modes plus one mode) behavior [27, 28] . The composition dependence of vLO and vTO for MgxZn1xSySe1y/GaAs is shown in Figure 4.12. The experimental data were obtained by Raman scattering [29]. In brief, we can expect four-mode behavior (AB-, AC-, BC- and BD-like) in an AxB1xCyD1y alloy. However, the data in Figure 4.12 reveal three-mode behavior (MgSe-, ZnSe- and MgZnS-like). Similarly,

112

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.11 Long-wavelength optical phonon frequencies vLO and vTO versus x for ZnSexTe1x at 300 K. [Reprinted with permission from Physica B, Infrared studies and optical characterization of ZnSe1xTex molecular beam epitaxial films by T. R. Yang and C. C. Lu, 284–288, 1187. Copyright (2000), Elsevier] The open circles represent the InP data 400 LO (MgZnS)

ω LO, TO (cm-1)

350 LO (MgSe)

300 LO

250 ZnSe-like 200

TO

Mgx Zn1-x S y Se1-y /GaAs

150

0

0.2

0.4

0.6

0.8

1.0

y

Figure 4.12 Long-wavelength optical phonon frequencies vLO and vTO versus y (S) for MgxZn1xSySe1y/GaAs at 300 K. [Reprinted with permission from D. Wang et al., J. Appl. Phys. 80, 1248 (1996). Copyright (1996), American Institute of Physics]

MgxZn1xSeyTe1y showed two-mode behavior (MgSeTe- and ZnSeTe-like), not four-mode behavior [30]. As expected, both ZnxCd1xHg1xyTe and CdSxSe1xTe1xy exhibited threemode behavior (Table 4.5).

4.2.3 External Perturbation Effect (a) Group-IV semiconductor alloy The phonon frequency is dependent both on temperature T and pressure p. The longwavelength optical phonon frequency vop versus T can be expressed as [31] vop ðTÞ ¼ vop ð0Þ

aT 2 T þb

ð4:7Þ

LATTICE DYNAMIC PROPERTIES

113

Figure 4.13 Hydrostatic-pressure dependence of the optical phonon frequency vop for Si0.55Ge0.45 at 300 K. The experimental data are taken from Sui et al. [32]. The bulk Si and Ge data are taken from Adachi [33]

where vop(0) is the T ¼ 0 K value, a is in cm1 per degree Kelvin and b is a quantity proportional to the Debye temperature (in Kelvins). No detailed data on the temperature dependence of vop ¼ vLO,TO in group-IV semiconductor alloys has been reported. The pressure dependence of vop in Si0.55Ge0.45 determined by Raman scattering is shown in Figure 4.13. The experimental data are taken from Sui et al. [32]. The pressure coefficients dv/ dp obtained from these plots are 7, 5 and 4 cm1/GPa for the SiSi, SiGe and GeGe modes, respectively. The solid lines in Figure 4.13 show the bulk Si and Ge data [33]. (b) III–V semiconductor alloy Figure 4.14 (a) shows the vLO versus T plots for the GaAs-like mode in AlxGa1xAs. The experimental data are taken from Jimenez et al. [34]. The temperature variations are almost linear in the range between 300 and 650 K. The corresponding coefficient dvLO/dT for AlxGa1xAs is plotted in Figure 4.14 (b) [34]. The GaAs (x ¼ 0) and AlAs (x ¼ 1.0) data are also shown by the solid and open triangles, respectively [35]. It can be seen that the temperature coefficients are almost composition independent (dvLO/dT2 102 cm1/K). The pressure dependence of the LO phonon frequencies in Al0.58Ga0.42As is shown in Figure 4.15. The LO phonon frequencies were measured by Raman scattering up to 7 GPa [36]. The pressure coefficients for the LO and TO modes in AlAs and GaAs were reported to be 5 (AlAs) and 4 cm1/GPa (GaAs), respectively [36]. The slopes for the experimental Al0.58Ga0.42As data in Figure 4.15 are nearly the same as those for AlAs and GaAs. The pressure coefficients dvLO,TO/dp for the AlAs- and GaAs-like LO and TO modes for AlxGa1xAs are plotted as a function of x in Figure 4.16. The experimental data are taken from Holtz et al. [36]. Although the experimental data largely scatter, we can see that they fall in the range 5.3 1.3 cm1/GPa, as shown by the vertical bar.

114

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.14 (a) Temperature dependence of the GaAs-like LO phonon frequency vLO for AlxGa1xAs. The data for bulk GaAs are also shown. [From J. Jimenez, E. Martın, A. Torres, and J. P. Landesman, Phys. Rev. B 58, 10463–10469 (1998). Copyright (1998) American Physical Society.] (b) Temperature coefficient dvLO/dT versus x for AlxGa1xAs at 300 K. The experimental data are taken from Jimenez et al. [34]. The solid and open triangles represent the endpoint binary data taken from Adachi [35]

Figure 4.15 Hydrostatic-pressure dependence of the AlAs- and GaAs-like LO phonon frequencies for Al0.58Ga0.42As at 300 K. The experimental data are taken from Holtz et al. [36]. The bulk GaAs data are also taken from Adachi [35]

LATTICE DYNAMIC PROPERTIES

115

dω LO,TO /dp (cm-1/GPa)

8 7 6 5 4 3 2

LO (AlAs) TO (AlAs) LO (GaAs) TO (GaAs)

AlxGa1-x As

1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.16 Pressure coefficients dvLO,TO/dT for the AlAs- and GaAs-like LO and TO modes in AlxGa1xAs at 300 K. The experimental data are taken from Holtz et al. [36]. The vertical bar indicates the range of the pressure-coefficient 5.3 1.3 cm1/GPa 400

LO (GaP) ω LO (cm-1)

380 360

LO (InP) LO (bulk InP)

340

Ga 0.5In0.5P 320

0

200

400

600

800

1000

T (K)

Figure 4.17 GaP- and InP-like LO phonon frequencies versus temperature T for Ga0.5In0.5P. The experimental data are taken from Shealy and Wicks [37]. The bulk InP data are also taken from Adachi [35]

The GaP- and InP-like LO phonon frequencies versus temperature T for Ga0.5In0.5P are plotted in Figure 4.17. The experimental data were measured by Raman spectroscopy [37]. The bulk InP vLO(T) values which were calculated from Equation (4.7) with vLO(0) ¼ 348.3 cm1, a ¼ 2.8 102 cm1/K and b ¼ 420 K are also shown [35]. The temperature variation in GaxIn1xP is found to be nearly the same as that in InP. The pressure dependence of the GaP- and GaAs-like LO and TO data for GaP0.11As0.89 is shown in Figure 4.18. The experimental data are taken from Galtier et al. [38]. The solid lines represent the bulk LO and TO values versus p for GaP and GaAs taken from Adachi [35]. The GaP0.11As0.89 data are found to be very similar to those for GaP. (c) II–VI semiconductor alloy The temperature variations of the LO and TO phonon frequencies vLO and vTO for c-ZnxCd1xSe are shown in Figure 4.19. The experimental data are taken from Valakh et al. [39]. The LO phonons in c-ZnxCd1xSe exhibit one-mode behavior, while the

116

PROPERTIES OF SEMICONDUCTOR ALLOYS 500 GaP0.11 As0.89

ω LO, TO (cm-1)

450

LO (bulk GaP)

400 350

LO (bulk GaAs) TO (bulk GaP)

300 TO (GaAs)

250

0

2

4

6

8

10

12

p (GPa)

Figure 4.18 Hydrostatic-pressure dependence of the GaP-like LO (solid circles) and TO phonon frequencies (open circles) in GaP0.11As0.89 at 85 K. The experimental data are taken from Galtier et al. [38]. The solid lines represent the bulk GaP and GaAs data taken from Adachi [35]

TO phonon branch is much more complicated. The resulting optical phonon behavior in c-ZnxCd1xSe is of the intermediate type, neither one-mode nor two-mode behavior. The experimental vLO versus T behavior in Figure 4.19 can be found in many ANB8N tetrahedral semiconductors. On the other hand, the effect of resonant interaction of the onephonon (TO) and two-phonon (2TA) states in c-ZnxCd1xSe [39] leads not only to the peculiar temperature dependence of intensity and line-shape of the bands, but also to the temperature

Figure 4.19 Temperature dependence of the LO and TO phonon frequencies vLO and vTO in c-ZnxCd1xSe. [Reprinted with permission from M. Y. Valakh et al., Phys. Status Solidi B 113, 635 (1982), Copyright (1982) Wiley–VCH]

LATTICE DYNAMIC PROPERTIES

117

300

LO (bulk ZnSe)

ω LO (cm -1)

280

260

LO (Zn 0.68 Cd 0.32 Se)

240

TO (bulk ZnSe)

220

200

0

2

4

6 p (GPa)

8

10

Figure 4.20 Hydrostatic-pressure dependence of the LO phonon frequency for Zn0.68Cd0.32Se layer grown on GaAs(100) measured at 300 K. The experimental data are taken from Li et al. [40]. The solid line shows the result calculated using Equation (4.8) (Zn0.68Cd0.32Se). The bulk ZnSe LO and TO phonon frequencies are obtained from Adachi [41]

shift of the phonon frequencies. The latter can be easily identified in Figure 4.19. The ordinary temperature shift in vLO takes place for x 0.75 for which the resonant interaction is small. When this interaction is significant (0.4 < x < 0.6), the phonon frequency vTO exhibits anomalous dependence on temperature; i.e. at x ¼ 0.50 and 0.58 vTO is practically unchanged over a wide temperature range from 100 to 450 K (Figure 4.19). This is due to the strengthening of anharmonic coupling with increasing temperature and, as a result, to the stronger repulsion effect of the TO and 2TA bands [39]. The pressure dependence of vLO for Zn0.68Cd0.32Se layer on GaAs(100) is shown in Figure 4.20. The Raman spectra were recorded up to 7 GPa [40]. The solid line represents the experimental data (vLO in cm1, p in GPa) vLO ðpÞ ¼ 241:07 þ 4:066p

ð4:8Þ

Also shown in Figure 4.20 are the experimental results for ZnSe [41] (vLO,TO in cm1, p in GPa) vLO ðpÞ ¼ 251:9 þ 3:44p0:02p2

ð4:9aÞ

vTO ðpÞ ¼ 204:2 þ 4:98p0:07p2

ð4:9bÞ

The pressure dependence of the ZnSe-like LO and TO phonon frequencies for MBE-grown ZnSe0.96Te0.04 layer is shown in Figure 4.21. The optical phonon frequencies were obtained by

118

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 4.21 Hydrostatic-pressure dependence of the ZnSe-like LO and TO phonon frequencies for ZnSe0.96Te0.04 at 300 K. [Reprinted with permission from C. S. Yang et al., Phys. Rev. B 59, 8128–8131 (1999). Copyright (1999) American Physical Society]

Raman scattering and FTIR measurements under pressures of up to 20 GPa [42]. Both ZnxCd1xSe (Figure 4.19) and ZnSexTe1x exhibit an intermediate-mode behavior (Table 4.5). In addition to the usual ZnSe-like LO and TO modes, a new LO–TO phonon pair can therefore be identified inside the reststrahlen band in ZnSexTe1x [25]. The ZnSe-like LO phonon frequency in Figure 4.21 can be approximated as (vLO in cm1, p in GPa) vLO ðpÞ ¼ 250 þ 3:3p

ð4:10Þ

On the other hand, the ZnSe-like TO phonon frequency exhibits anomalous dependence on p, i.e. it increases almost linearly up to 3 GPa and tends to show a saturated value of 225 cm1 for p > 3 GPa. There have been many Raman peaks observed in ZnSexTe1x for 0 < x < 1.0 between the ZnSe-like LO and TO phonon frequency region. The anomalous pressure dependence of the ZnSe-like TO phonon frequency may be correlated with this fact [42]. Raman scattering has been used to investigate anharmonicity and disorder-induced effects in MBE-BexZn1xSe/GaAs(100) epilayers [43]. The anharmonicity is found to be higher in BexZn1xSe than in ZnSe, increasing with compositional disorder. In conclusion of this section, the temperature and pressure coefficients of the longwavelength optical phonon frequencies dvop/dT (or v1 op dvop =dT ¼ d lnvop =dT) and dvop/ dp (or v1 op dvop =dp ¼ d lnvop =dp) in alloys of exhibiting one-mode behavior can be simply estimated from the linear interpolation between the endpoint values. In the case of two-mode (three- or four-mode) behavior in group-IV binaries and in III–V and II–VI ternaries (quaternaries), the temperature and pressure coefficients of the endpoint material values can be used, to a first approximation, as those for each phonon mode. For example, in an AxB1xC alloy, the temperature coefficient of the AC-like (BC-like) LO phonon frequency is the same as that of the bulk material AC (BC). These are schematically shown in Figure 4.22. A variety of the endpoint material data can be found in Adachi [33, 35, 41].

LATTICE DYNAMIC PROPERTIES

119

LO (AC) LO dωop /dT, dωop /dp

TO (AC)

TO

LO (BC) TO (BC) AxB1-xC

(a) one-mode 0

0.2

0.4

(b) two-mode 0.6

0.8

1.0 0

x

0.2

0.4

0.6

0.8

1.0

x

Figure 4.22 Schematic representations of the composition dependence of the temperature and pressure coefficients, dvop/dT and dvop/dp, in an alloy of composition AxB1xC (solid lines). The solid and open circles represent the endpoint binary data. The dependence of vop on x is also schematically shown by the dashed lines. The schemes represented by the solid lines can also be used for estimating mode Gr€ uneisen parameters and PDPs

€ 4.3 MODE GRUNEISEN PARAMETER The anharmonic properties of solids are customarily described in terms of the Gr€uneisen parameter g. As a measure of the volume dependence of the phonon frequency ni(q) of the ith mode, the mode Gr€ uneisen parameter g i(q) can be defined by g i ðqÞ ¼

d½lnni ðqÞ V dni ðqÞ ¼ d½lnV ni ðqÞ dV

ð4:11Þ

where V is the crystal volume. The mode Gr€ uneisen parameters for the long-wavelength (q ¼ 0) phonons in some non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Tables 4.5 and 4.6 of Adachi [31]. Figure 4.23 shows the g parameters for (a) SiSi, (b) SiGe and (c) GeGe modes in SixGe1x. The experimental data are taken from Sui et al. [32]. The Si and Ge values are also taken from Adachi [33]. The SiSi (GeGe) mode parameter slightly decreases (increases) with increasing x, while the SiGe mode parameter is nearly independent of x. The LO and TO phonon g parameters versus x for AlxGa1xAs are plotted in Figure 4.24. The alloy data are taken from Holtz et al. [36]. The binary data are also taken from Adachi [35]. These data scatter relatively largely, but show no strong dependence on x. They fall in the range g LO,TO ¼ 1.1 0.3, as indicated by the vertical bar. Figure 4.25 plots the mode Gr€ uneisen parameter g versus x for c-GaNxAs1x. The experimental data are taken from G€ ungerich et al. [44]. These authors used the pressure-dependent shift of the GaAs-like local vibrational mode to calculate the

120

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.6 γ

1.4 1.2 SixGe1-x

1

(a) Si-Si

0.8 1.6 γ

1.4 1.2 1

(b) Si-Ge

0.8 1.6 γ

1.4 1.2 1

(c) Ge-Ge

0.8 0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.23 Mode Gr€uneisen parameters g versus x for (a) SiSi, (b) SiGe and (c) GeGe phonon pairs in SixGe1x at 300 K. The experimental data are taken from Sui et al. [32]. The endpoint elemental data are also taken from Adachi [33]

anharmonicity of the GaN bond potential and qualitatively confirmed the simple picture in which the GaN bonds are significantly overstretched in Ga(N, As) with respect to their equilibrium length realized in GaN. Finally, the composition dependence of the mode Gr€uneisen parameter in various semiconductor alloys can be estimated, to a first approximation, from the scheme shown in Figure 4.22. Using an AxB1xC alloy that exhibits the two-mode behavior as an example, the AC-like LO phonon mode has the same Gr€ uneisen parameter as that of AC, irrespective of x. Similarly, the BC-like LO phonon mode has the same Gr€uneisen parameter as that of BC 2.1 1.8

AlxGa1-x As

1.5 γ

1.2 0.9

LO (AlAs) TO (AlAs) LO (GaAs) TO (GaAs)

0.6 0.3 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.24 Mode Gr€uneisen parameter g versus x for AlxGa1xAs at 300 K. The experimental data are taken from Holtz et al. [36]. The endpoint binary data are also taken from Adachi [35] (solid and open squares). The vertical bar indicates the range of g LO,TO ¼ 1.1 0.3

LATTICE DYNAMIC PROPERTIES

121

2.1 1.8

c-GaNx As1-x

γ

1.5 1.2 0.9 0.6

LO (GaAs) TO (GaAs)

0.3 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.25 Mode Gr€uneisen parameter g versus x for c-GaNxAs1x at 300 K. The experimental data are taken from G€ungerich et al. [44]

(Figure 4.22(b)). The endpoint g values for some non-alloyed group-IV, III–V and II–VI semiconductors can be found in Adachi [31,33,35,41].

4.3.1 Phonon Deformation Potential Strain- or stress-induced shift of the phonon frequency can be explained by the PDP [31]. The PDPs for some non-alloyed group-IV, III–Vand II–VI semiconductors are summarized in Adachi [31, 33, 35, 41]. A very few data have, however, been reported on alloy materials. This necessitates the use of some sort of an interpolation scheme. The interpolation scheme in Figure 4.22 may be the simplest and most reliable way to estimate alloy PDP values. Indeed, the GaN- and AlN-like E2 (high) phonon modes in w-AlxGa1xN have the same PDPs as the relevant endpoint binary values (w-GaN and w-AlN), respectively. [45]. The strain («)-induced shift of the LO phonon frequency can now be given by C12 S12 DvLO « ¼ vLO K12 ðLOÞ K11 ðLOÞ « ¼ vLO K12 ðLOÞ þ K11 ðLOÞ « C11 S11 þ S12 ð4:12Þ where Kij is the dimensionless PDP and Cij (Sij) is the elastic stiffness (compliance) constant. The Kij is usually defined, using p and q, as [31] K11 ¼

p ; v2LO

K12 ¼

q v2LO

ð4:13Þ

Equation (4.12) can, then, be rewritten as DvLO « ¼

1 C12 1 S12 qðLOÞ pðLOÞ « ¼ qðLOÞ þ pðLOÞ « b« ð4:14Þ vLO vLO C11 S11 þ S12

The b versus x data for SixGe1x are shown in Figure 4.26. The experimental data are taken from Lockwood and Baribeau [46] (open circles), Stoehr et al. [47] (open squares),

122

PROPERTIES OF SEMICONDUCTOR ALLOYS

b (cm-1)

-300 -600 -900 -1200

(a) Si-Si

b (cm-1)

-1500 -300 -600 -900 -1200

(b) Si-Ge

b (cm-1)

-1500 0 -300

(c) Ge-Ge

-600 -900 -1200

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.26 Optical-phonon strain-shift coefficient b versus x for SixGe1x at 300 K. The experimental data are taken from Lockwood and Baribeau [46] (open circles), Stoehr et al. [47] (open squares), Wong et al. [48] (open triangles) and Pezzoli et al. [49] (solid circles). The solid lines represent the linear leastsquares fit of these data

Wong et al. [48] (open triangles) and Pezzoli et al. [49] (solid circles). It can be seen that the SiGe and GeGe modes gradually decrease with increasing x, while the SiSi mode is nearly independent of x. However, Reparaz et al. [50] were unable to observe any clear composition dependence of the Si-like, Ge-like and SiGe modes in SixGe1x between x ¼ 0 and 0.6. The GaP- and GaAs-like LO-phonon coefficients b for GaPxAs1x are shown in Figure 4.27. The experimental data correspond to those for the (001) biaxial strain [51]. A much higher frequency shift of the GaAs-like mode than that of the GaP-like mode can be seen, suggesting

0 GaPx As1-x b (cm-1)

-300 LO (GaP)

-600 LO (GaAs)

-900 -1200

0

0.2

0.4

0.6

0.8

1.0

x

Figure 4.27 GaP- and GaAs-like LO-phonon strain-shift coefficients b versus x for GaPxAs1x at 300 K. The experimental data are taken from Armelles et al. [51]. The solid lines represent the linear leastsquares fit (in cm1): b ¼ 308–437x (GaP-like) and 513–1069x (GaAs-like)

LATTICE DYNAMIC PROPERTIES

123

that the biaxial strain is not accommodated in the same way by the two types of bonds in GaPxAs1x.

REFERENCES [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32]

C. W. Myles, Phys. Rev. B 28, 4519 (1983). S. Baroni, S. de Gironcoli, and P. Giannozzi, Phys. Rev. Lett. 65, 84 (1990). J. A. Kash, J. M. Hvam, J. C. Tsang, and T. F. Kuech, Phys. Rev. B 38, 5776 (1988). G. P. Srivastava, The Physics of Phonons. Adam Hilger, Bristol, (1990). I. F. Chang and S. S. Mitra, Adv. Phys. 20, 359 (1971). I. F. Chang and S. S. Mitra, Phys. Rev. 172, 924 (1968). A. Mascarenhas, H. M. Cheong, M. J. Seong, and F. Alsina, in Spontaneous Ordering in Semiconductor Alloys (edited by A. Mascarenhas), Kluwer Academic, New York, 2002, p. 391. F. Pezzoli, L. Martinelli, E. Grilli, M. Guzzi, S. Sanguinetti, M. Bollani, H. D. Chrastina, G. Isella, H. von K€anel, E. Wintersberger, J. Stangl, and G. Bauer, Mater. Sci. Eng. B 124–125, 127 (2005). J. C. Tsang, V. P. Kesan, J. L. Freeouf, F. K. LeGoues, and S. S. Iyer, Phys. Rev. B 46, 6907 (1992). M. Melendez-Lira, J. Menendez, W. Windl, O. F. Sankey, G. S. Spencer, S. Sego, R. B. Culbertson, A. E. Bair, and T. L. Alford, Phys. Rev. B 54, 12866 (1996). B.-K. Yang, M. Krishnamurthy, and W. H. Weber, J. Appl. Phys. 84, 2011 (1998). L. V. Kulik, C. Guedj, M. W. Dashiell, J. Kolodzey, and A. Hairie, Phys. Rev. B 59, 15753 (1999). H. Harima, T. Inoue, S. Nakamura, H. Okumura, Y. Ishida, S. Yoshida, T. Koizumi, H. Grille, and F. Bechstedt, Appl. Phys. Lett. 74, 191 (1999). A. Tabata, J. R. Leite, A. P. Lima, E. Silveira, V. Lemos, T. Frey, D. J. As, D. Schikora, and K. Lischka, Appl. Phys. Lett. 75, 1095 (1999). K. Torii, N. Usukura, A. Nakamura, T. Sota, S. F. Chichibu, T. Kitamura, and H. Okumura, Appl. Phys. Lett. 82, 52 (2003). B. Jusserand, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 30. Z. C. Feng, S. Perkowitz, R. Rousina, and J. B. Webb, Can. J. Phys. 69, 386 (1991). M. H. Brodsky, G. Lucovsky, M. F. Chen, and T. S. Plaskett, Phys. Rev. B 2, 3303 (1970). S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP. John Wiley & Sons, Ltd, New York, 1992. T. Sugiura, N. Hase, Y. Iguchi, and N. Sawaki, Jpn. J. Appl. Phys. 37, 544 (1998). R. Manor, O. Brafman, and R. F. Kopf, Phys. Rev. B 56, 3567 (1997). G. Lucovsky, E. Lind, and E. A. Davis, in II–VI Semiconducting Compounds (edited by D. G. Thomas), Benjamin, New York, 1967, p. 1150. J. Baars and F. Sorger, Solid State Commun. 10, 875 (1972). M. P. Volz, F. R. Szofran, S. L. Lehoczky, and C. -H. Su, Solid State Commun. 75, 943 (1990). T. R. Yang and C. C. Lu, Physica B 284–288, 1187 (2000). R. G. Alonso, E.-K. Suh, A. K. Ramdas, N. Samarth, H. Luo, and J. K. Furdyna, Phys. Rev. B 40, 3720 (1989). O. Pages, T. Tite, D. Bormann, O. Maksimov, and M. C. Tamargo, Appl. Phys. Lett. 80, 3081 (2002). O. Pages, M. Ajjoun, T. Tite, D. Bormann, E. Tournie, and K. C. Rustagi, Phys. Rev. B 70, 155319 (2004). D. Wang, D. Huang, C. Jin, X. Liu, Z. Lin, J. Wang, and X. Wang, J. Appl. Phys. 80, 1248 (1996). H. Makino, H. Sasaki, J. H. Chang, and T. Yao, J. Cryst. Growth 214/215, 359 (2000). S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. Z. Sui, H. H. Burke, and I. P. Herman, Phys. Rev. B 48, 2162 (1993).

124

PROPERTIES OF SEMICONDUCTOR ALLOYS

[33] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [34] J. Jimenez, E. Martın, A. Torres, and J. P. Landesman, Phys. Rev. B 58, 10463 (1998). [35] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [36] M. Holtz, M. Seon, O. Brafman, R. Manor, and D. Fekete, Phys. Rev. B 54, 8714 (1996). [37] J. R. Shealy and G. W. Wicks, Appl. Phys. Lett. 50, 1173 (1987). [38] P. Galtier, J. Chevallier, M. Zigone, and G. Martinez, Phys. Rev B 30, 726 (1984). [39] M. Y. Valakh, M. P. Lisitsa, G. S. Pekar, G. N. Polysskii, V. I. Sidorenko, and A. M. Yaremko, Phys. Status Solidi B 113, 635 (1982). [40] W. S. Li, Z. X. Shen, D. Z. Shen, and X. W. Fan, J. Appl. Phys. 84, 5198 (1998). [41] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [42] C. S. Yang, W. C. Chou, D. M. Chen, C. S. Ro, J. L. Shen, and T. R. Yang, Phys. Rev. B 59, 8128 (1999). [43] L. Y. Lin, C. W. Chang, W. H. Chen, Y. F. Chen, S. P. Guo, and M. C. Tamargo, Phys. Rev. B 69, 075204 (2004). [44] M. G€ungerich, P. J. Klar, W. Heimbrodt, J. Koch, W. Stolz, M. P. Halsall, and P. Harmer, Phys. Rev. B 71, 075201 (2005). [45] A. Sarua, M. Kuball, and J. E. Van Nostrand, Appl. Phys. Lett. 85, 2217 (2004). [46] D. J. Lockwood and J.-M. Baribeau, Phys. Rev. B 45, 8565 (1992). [47] M. Stoehr, D. Aubel, S. Juillaguet, J. L. Bischoff, L. Kubler, D. Bolmont, F. Hamdani, B. Fraisse, and R. Fourcade, Phys. Rev. B 53, 6923 (1996). [48] L. H. Wong, C. C. Wong, J. P. Liu, D. K. Sohn, L. Chan, L. C. Hsia, H. Zang, Z. H. Ni, and Z. X. Shen, Jpn. J. Appl. Phys. 44, 7922 (2005) . [49] F. Pezzoli, E. Bonera, E. Grilli, M. Guzzi, S. Sanguinetti, D. Chrastina, G. Isella, H. von K€anel, E. Wintersberger, J. Stangl, and G. Bauer, J. Appl. Phys. 103, 093521 (2008). [50] J. S. Reparaz, A. Bernardi, A. R. Gon~i, M. I. Alonso, and M. Garriga, Appl. Phys. Lett. 92, 081909 (2008). [51] G. Armelles, M. J. Sanjuan, L. Gonzalez, and Y. Gonzalez, Appl. Phys. Lett. 68, 1805 (1996).

5 Collective Effects and Some Response Characteristics 5.1 PIEZOELECTRIC CONSTANT 5.1.1 General Considerations A crystal with a center of symmetry cannot be piezoelectric [1]. Thus, the diamond-type crystals (diamond, Si, Ge and a-Sn) cannot be piezoelectric. Tables 5.1 and 5.2 summarize the piezoelectric constants for some ANB8N tetrahedral semiconductors with cubic and hexagonal crystal structures, respectively. Note that the piezoelectric strain constant dij is connected reciprocally with the stress constant eik in the following manner dij ¼

X

eik Skj

ð5:1Þ

dik Ckj

ð5:2Þ

k

or, vice versa eij ¼

X k

where Skj (Ckj) is the elastic compliance (stiffness) constant [1].

5.1.2 Alloy Value Figure 5.1 shows the plot of e14 versus x for CxSi1x. The theoretical e14 value for 3C-SiC is 0.345 C/m2 [2]. However, no experimental e14 data for 3C-SiC has been reported. Similarly, SixGe1x will in principle have a nonzero e14 value at an ordered phase x 0.5. In the fully disordered group-IV semiconductor alloys (CxSi1x, SixGe1x, etc.), we have zero e14 values over the whole alloy range 0 x 1.0. Using the endpoint binary data in Table 5.2, the liner interpolation scheme provides a set of the piezoelectric constants eij for w-AlxGa1xN (in C/m2) e15 ðxÞ ¼ 0:330:15x

ð5:3aÞ

e31 ðxÞ ¼ 0:550:03x

ð5:3bÞ

e33 ðxÞ ¼ 1:12 þ 0:43x

ð5:3cÞ

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

126

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 5.1 Piezoelectric stress and strain constants, e14 and d14, for some cubic group-IV, III–Vand II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt e14 (C/m2)

d14 (1012 m/V)

Diamond (d)a Si (d)a Ge (d)a Sn (d)a 3C-SiC (zb)

0 0 0 0 0.345b

0 0 0 0 1.35b

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

1.04b 0.36b 1.13b 0.06b 0.23b 0.068 0.61b 0.10 0.16 0.126 0.71b 0.083 0.045 0.071

System

Material

IV

III–V

II–VI

a b

MgO (rs)a ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs)a CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

0 0.147 0.049 0.028 0 0.37b 0.27b 0.0335 0.14b 0.058b 0.029b

9.7b 3.9b 1.7 6.4b 1.42 2.7 2.92 1.80 1.14 2.4 0 3.18 1.10 0.91 0 1.68 5.3b 2.6b 1.4b

Principally showing no piezoelectricity Estimated or calculated

The piezoelectric properties of ordered and disordered IIIN alloys have been theoretically studied by several authors [3,4]. The piezoelectric constant e33 versus x for w-GaxIn1xN is reproduced in Figure 5.2 [4]. The solid line shows the x dependence of e33 for disordered w-GaxIn1xN, while the solid circles refer to ordered values. Four ordered structures, all exhibiting ordering along the c axis, will be considered. The first structure is denoted 1 1 and consists of a single Ga plane alternating with a simple In plane. This structure has also been studied by Bernardini and Fiorentini [3] and has an overall composition x ¼ 0.5. The second structure, denoted 2 2, also has an overall composition of 50 at% but

COLLECTIVE EFFECTS AND SOME RESPONSE CHARACTERISTICS

127

Table 5.2 Piezoelectric stress and strain constants eij and dij for some hexagonal group-IV, III–V and II–VI semiconductors. w ¼ wurtzite; h ¼ hexagonal (P63/mmc (D6h)) System

eij (C/m2)

Material

dij (1012 m/V)

e31

e15 IV

2H-SiC (w)

0.08a

III–V

BN (h)b AlN (w) GaN (w) InN (w)

0 0.48 0.33c

II–VI

BeO (w) ZnO (w) ZnS (w) CdS (w) CdSe (w)

e33

d15

d31

d33

0.2a

0.37 0.118 0.183 0.138

0 0.58 0.55 0.41c

0 1.55 1.12 0.81c

0.051 0.62 0.238 0.262 0.160

0.092 0.96 0.265 0.385 0.347

0 4.07 3.1

0 2.65 1.9

0 5.53 3.7 4.7

8.3 4.37 11.91 10.51

0.12 5.12 2.14 5.09 3.92

0.24 12.3 3.66 9.71 7.84

Assuming that the 2H-SiC values are the same as those for 6H-SiC within experimental error Principally showing no piezoelectricity c Estimated or calculated a b

e14 (C/m2)

0

CxSi1-x

-0.1

Disordered alloy

Ordered alloy

-0.2 -0.3

3C-SiC

-0.4 -0.5

0

0.2

0.4

x

0.6

0.8

1.0

Figure 5.1 Piezoelectric stress constant e14 versus x for CxSi1x. The open circles show the endpoint elemental data (e14 ¼ 0), while the solid circle refers to the theoretical 3C-SiC (x ¼ 0.5) value

Figure 5.2 Theoretical piezoelectric stress constant e33 versus x for w-GaxIn1xN. The solid line shows the disordered alloy values, while the solid circles plot the ordered values. [Reprinted with permission from A. Al-Yacoub, L. Bellaiche, and S.-H. Wei, Phys. Rev. Lett. 89, 7601–7604 (2002). Copyright (2002) American Physical Society]

128

PROPERTIES OF SEMICONDUCTOR ALLOYS

differentiates itself from the 1 1 structure by exhibiting two pure Ga planes alternating with two pure In planes. The third (respectively, fourth) structure exhibits a succession of three (respectively, one) Ga and one (respectively, three) In planes. Consequently, it is denoted as 3 1 (respectively, 1 3) while having a Ga composition of 75 at% (respectively, 25 at%). The theoretical results in Figure 5.2 indicate that the atomic ordering can have a large effect on the piezoelectricity and that e33 of disordered alloys is nearly linear with respect to x. The simple linear interpolation scheme, using the endpoint binary data in Table 5.2, provides e33 for w-GaxIn1xN (in C/m2) e33 ðxÞ ¼ 0:81 þ 0:31x

ð5:4Þ

Equation (5.4) indicates an increase in e33 with increasing x, in direct contrast to that obtained in Figure 5.2 [4]. Figure 5.3 shows the piezoelectric constant e14 as a function of x for GaxIn1xAs. The experimental data are taken from Sanchez-Rojas et al. [5] (solid circles), Chan et al. [6] (open square) and Izpura et al. [7] (open triangle). The solid line is obtained from the linear interpolation scheme between the endpoint data (open circles). It can be seen from Figure 5.3 that e14 passes through zero at x 0.2 while undergoing a reversal in sign. The experimental data are slightly larger than the linearly interpolated values. 0.08

e14 (C/m2)

0.04 0 -0.04 -0.08 Gax In1-x As

-0.12 -0.16 -0.20

0

0.2

0.4

x

0.6

0.8

1.0

Figure 5.3 Piezoelectric stress constant e14 versus x for GaxIn1xAs. The experimental data are taken from Sanchez-Rojas et al. [5] (solid circles), Chan et al. [6] (open square) and Izpura et al. [7] (open triangle). The solid line represents the linearly interpolated result between the endpoint binary data

No experimental data on alloy eij values have been reported, except for GaxIn1xAs (Figure 5.3). The piezoelectric constants e14 for AlxGa1xAs and GaxIn1xPyAs1y/InP in Figure 5.4 have been calculated from Equations (A.4) and (A.6), respectively, and can be given by e14 ðxÞ ¼ 0:23 þ 0:07x

ð5:5Þ

e14 ðyÞ ¼ 0:05 þ 0:15y0:18y2

ð5:6Þ

for AlxGa1xAs and

for GaxIn1xPyAs1y/InP.

COLLECTIVE EFFECTS AND SOME RESPONSE CHARACTERISTICS 0

129

0

e14 (C/m2)

(a) AlxGa1-x As -0.05

-0.05

-0.10

-0.10

-0.15

-0.15

-0.20

-0.20 (b) Ga xIn1-xPyAs1-y /InP

-0.25 0

0.2 0.4 0.6 0.8 1.0 x

-0.25 0

0.2 0.4 0.6 0.8 1.0 y

Figure 5.4 Piezoelectric stress constant e14 versus x or y for (a) AlxGa1xAs and (b) GaxIn1x PyAs1y/InP calculated from the linear interpolation scheme. The open circles show the endpoint binary data

€ 5.2 FROHLICH COUPLING CONSTANT 5.2.1 General Considerations The theory of Fr€ ohlich interaction in alloys of multi-mode phonon behaviors is very complex. Simply, it is possible to assume that there is a value for the Fr€ohlich coupling constant aF for each phonon mode given by pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ h=2mac vLO 1 1 e2 = 1 aF ¼ 2 «¥ «s vLO h

ð5:7Þ

where e is the electron charge, mac is the electron effective mass (conductivity mass), vLO is the LO phonon frequency and «¥ and «s are the high-frequency and static dielectric constants, respectively. The final alloy aF value can be obtained from the weighted average of each mode (i.e. Equation (5.7)). Nash et al. [8] discussed the Fr€ ohlich interaction in alloys of two-mode behavior based on a MREI model. They found that the electron–phonon coupling in In0.53Ga0.47As is much weaker for the InAs-like mode than for the GaAs-like mode. The primary reason for this was considered to be the coupling of the LO distortions by the macroscopic electric field. A theory of the Fr€ ohlich interaction in semiconductor alloys has also been proposed by several authors [9,10].

5.2.2 Alloy Value Table 5.3 summarizes the Fr€ ohlich coupling constant aF for some non-alloyed group-IV, III–V and II–VI semiconductors. The simplest way to obtain the alloy value is to use the linear interpolation scheme using the endpoint data in Table 5.3.

130

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 5.3 Fr€ohlich coupling constant aF for some group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite; rs ¼ rocksalt System

Material

aF

System

Material

aF

IV

Diamond (d)a Si (d)a Ge (d)a Sn (d)a 3C-SiC (zb)

0 0 0 0 0.256

II–VI

III–V

AlN (w) AlAs (zb) AlSb (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

0.65 0.126 0.023 0.48 0.201 0.068 0.025 0.24 0.15 0.0454 0.022

ZnO (w) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (w) CdSe (w) CdTe (zb)

1.19 0.63 0.432 0.332 0.75 0.514 0.46 0.35

a

Principally showing no Fr€ohlich coupling interaction

αF

The x dependence of aF for CxSi1x is shown in Figure 5.5. The Fr€ohlich coupling constant aF is strongly dependent on the ionic polarization of the crystal, which is related to the static and high-frequency dielectric constants «s and «¥. Note that «s is equal to «¥ in such diamondtype crystals. Thus, no Fr€ ohlich coupling occurs in diamond-type crystals (aF ¼ 0, see Equation (5.7)). 0.35 0.30 0.25 0.20 0.15 0.10 0.05 0

Cx Si1-x 3C-SiC

Ordered alloy

0

0.2

0.4

Disordered alloy

x

0.6

0.8

1.0

Figure 5.5 Fr€ohlich coupling constant aF versus x for CxSi1x. The open circles show the endpoint elemental data, while the solid circle refers to the experimental 3C-SiC (x ¼ 0.5) value

The aF value of 3C-SiC is 0.256 [11]. This means that the bond polarity of SiC resembles that of III–V and II–VI semiconductors (aF 6¼ 0) rather than that of Si or diamond (aF ¼ 0). Similarly, an alloy of SixGe1x will have a nonzero aF value near the ordered phase x 0.5, although this has never been confirmed experimentally. In the fully disordered alloys (CxSi1x, SixGe1x, etc.), a value of aF ¼ 0 can be expected over the whole alloy range 0 x 1.0.

COLLECTIVE EFFECTS AND SOME RESPONSE CHARACTERISTICS

131

0.20

αF

0.15

Gax In1-x Py As1-y /InP

0.10 0.05 0 0

0.2

0.4

0.6

0.8

1.0

y

Figure 5.6 Fr€ohlich coupling constant aF versus y for GaxIn1xPyAs1y/InP. The solid line shows the linear interpolation result of Equation (A.6), which can be successfully approximated by the quadratic expression shown in Equation (5.8). The open circle shows the InP data

The linearly interpolated aF value, obtained using Equation (A.6), is shown versus y for GaxIn1xPyAs1y/InP in Figure 5.6. This plot gives very weak upward bowing and can be expressed as aF ðyÞ ¼ 0:056 þ 0:107y0:013y2

ð5:8Þ

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] A. P. Mirgorodsky, M. B. Smirnov, E. Abdelmounıˆm, T. Merle, and P. E. Quintard, Phys. Rev. B 52, 3993 (1995). [3] F. Bernardini and V. Fiorentini, Phys. Rev. B 64, 085207 (2001); erratum, ibid. 65, 129903 (2002). [4] A. Al-Yacoub, L. Bellaiche, and S.-H. Wei, Phys. Rev. Lett. 89, 057601 (2002). [5] J. L. Sanchez-Rojas, A. Sacedon, F. Gonzalez-Sanz, E. Calleja, and E. Mu~ noz, Appl. Phys. Lett. 65, 2042 (1994). [6] C. H. Chan, Y. F. Chen, M. C. Chen, H. H. Lin, and G. J. Jan, J. Appl. Phys. 84, 1595 (1998). [7] I. Izpura, J. F. Valtue~na, J. L. Sanchez-Rojas, A. Saced on, E. Calleja, and E. Mu~ noz, Solid-State Electron. 40, 463 (1996). [8] K. J. Nash, M. S. Skolnick, and S. J. Bass, Semicond. Sci. Technol. 2, 329 (1987). [9] R. Zheng and M. Matsuura, Phys. Rev. B 59, 15422 (1999). [10] X. X. Liang and S. L. Ban, J. Lumin. 94–95, 781 (2001). [11] E. Kartheuser, in Polarons in Ionic Crystals and Polar Semiconductors (edited by J. T. Devreese), North-Holland, Amsterdam, 1972, p. 717.

6 Energy-band Structure: Energy-band Gaps 6.1 INTRODUCTORY REMARKS 6.1.1 Quasi-cubic Band Model The review in this chapter is concerned with the most important band-gap energies as a function of alloy composition. They are: E0, E0 þ D0, E1, E1 þ D1, E2, EgX , EgL , etc., and some of these gaps are shown in Figure 6.1 (see also Adachi [1]). In Figure 6.1, the fundamental absorption refers to band-to-band or to excitonic transitions. The fundamental absorption manifests itself by a rapid rise in absorption and can be used to determine the band-gap energy of semiconductors and insulators. In most semiconductors, the lowest direct band-gap transitions occur at the E0 edge, i.e. at the center of the BZ. Birman [2] discussed the relationship between the k ¼ 0 (G) CB and VB states of the wurtzite structure and the corresponding states of the zinc-blende structure. The essential difference between the potential that an electron experiences in an ideal wurtzite lattice and that in a zinc-blende lattice is the relatively small difference in ‘crystal field’ due to sites beyond the next nearest neighbors. Figure 6.2 shows the CB and VB states for (a) zinc-blende (Dso ¼ Dcr ¼ 0), (b) zinc-blende (Dso 6¼ 0, Dcr ¼ 0) and (c) wurtzite semiconductors at k ¼ 0. In the actual VB structure of a wurtzite crystal, the three VBs illustrated in Figure 6.2(c) can be thought of as arising from Figure 6.2(a) by the combined effect of both SO and crystal-field perturbations, while the wavefunction for each band may be written as a linear combination of px, py and pz and spin functions, provided the interaction of the G7 VB levels with the CB is neglected. This approach is known as the quasi-cubic model [3]. Under the SO interaction represented by the matrix element Dso and that of the crystal field represented by Dcr, the quasi-cubic model provides the difference in energies of the VBs DEBA ¼ E0B E0A

Dso þ Dcr ¼ 2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Dso þ Dcr 2 2 Dso Dcr 3 2

DECA ¼ E0C E0A

Dso þ Dcr þ ¼ 2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Dso þ Dcr 2 2 Dso Dcr 3 2

ð6:1aÞ

ð6:1bÞ

The lowest direct band-gap energies in wurtzite semiconductors can then be given by E0A, E0B and E0C, as shown in Figure 6.2(c). The lowest direct (E0) and lowest indirect gap energies (EgX , EgL ) for some group-IV, III–V and II–VI semiconductors are summarized in Table 6.1. Table 6.2 also lists the lowest direct Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

134

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 6.1 Electronic energy-band structure of Ge. The electronic states are labeled using the notation for the representations of the double group of the diamond structure. The main interband transitions are indicated by vertical arrows (at 300 K)

Zincblende Γ1

Wurtzite

Γ6

Γ7

E0 Γ15

E0A E0B

E0C

Γ9 (A)

Γ8 Γ7

(a) ∆so=∆cr=0

E0+∆0

∆so=∆0

(b) ∆cr=0

∆EBA

Γ7 (B) Γ7 (C)

∆ECA

(c) ∆so>0, ∆cr>0

Figure 6.2 Relationships between the VB splitting at the G point in the zinc-blende ((a) Dso ¼ Dcr ¼ 0, (b) Dso 6¼ 0, Dcr ¼ 0) and (c) wurtzite lattices (Dso 6¼ 0, Dcr 6¼ 0) and between the irreducible representations of the CB and VB in these lattices. (b) and (c) show the actual splitting found in the zinc-blende and wurtzite crystals, respectively

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

135

Table 6.1 E0, EgX and EgL for some cubic group-IV, III–V and II–VI semiconductors at 300 K. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

II–VI

BN (zb) BP (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb) BeS (zb) BeSe (zb) BeTe (zb) MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnO (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

Estimated At 1.5 K c At 4.2 K d Calculated or estimated e Tentative assignment f Estimated from AlxGa1xP data g Grown on MgO(100) substrate a b

E0 (eV) 15.3 4.06 0.795 0.413b 7.4 7.9–11.40d 5 1.45e 5.2 3.91f 3.01 2.27 3.231g 2.76 1.43 0.72 0.56 1.35 0.359 0.17 > 5.5 5.6 4.1 7.8 4.45 4.0 3.4 3.17 3.726 2.721 2.27 2.16 2.46 1.675 1.51 0.04 0.08 0.15

EgX (eV)

EgL (eV)

5.50 1.12 0.852

7.26a 2.0 0.6657 0.092c 4.20

2.39 6.27 2.0 5.34 2.48 2.15 1.615 4.2d 2.261 1.911 1.05 3.0d 2.21 1.37 1.63

8.6d 3.57d 2.37 2.211 5.5d 2.63 1.72 0.76 5.8d 2.05 1.07 0.93

4–4.5 2.63 3.6d 3.2d 2.5d 5.14d 3.4 3.05 5.24d 4.37d 3.48d

3.8

136

PROPERTIES OF SEMICONDUCTOR ALLOYS

gaps E0A, E0B and E0C for some wurtzite-type group-IV, III–V and II–VI semiconductors. The Dso and Dcr values can be seen in Table 6.6 of Adachi [1].

6.1.2 Bowing Parameter In a conventional band-structure calculation, the electrons are assumed to be independent particles interacting with some average potential due to positively charged ions and valence electrons, at an equilibrium lattice constant a. Since the electron wavefunction in a strictly periodic function must be of the form exp(ikr)uk(r), where uk(r) is a periodic function which satisfies the periodic boundary conditions, it is convenient to compute electron energies E as a function of k. The computed energies are then drawn for various values of the wavevector lying along high symmetry lines in the first BZ (Figure 6.1). Though an alloy has no translational invariance, the VCA can recover it by replacing the potential by a periodic one, which is produced by ‘average’ atoms. For an AlxGa1xAs alloy, the potential is approximated by uVCA(r) ¼ xuAlAs(r) þ (1 x)uGaAs(r), which is periodic. The band-gap energy is a typical case exhibiting nonlinearity with respect to alloy composition. Van Vechten and Bergstresser [4] developed a physical model for obtaining the bowing parameter of E0 based on the Phillips’s dielectric theory of electronegativity [5]. The deviation from linearity is considered to be due to two terms involving ci, the intrinsic bowing parameter due to the VCA, and ce, the extrinsic bowing parameter due to aperiodicity in the alloy lattice c ¼ ci þ ce

ð6:2Þ 2 CA-B ,

i.e. to the square of the The extrinsic term ce can be taken to be proportional to electronegativity difference CA-B between the atoms A and B in an AxB1xC alloy.

6.1.3 Ordered Alloy As mentioned in Section 1.3.2, it has become evidence that many cubic semiconductor alloys can exhibit spontaneous ordering. For example, Ga0.5In0.5P, when grown under proper conditions, forms the CuPt-B ordered structure. In this structure, an alternate GaP/InP monolayer SL is formed along the h111i direction. The effects of atomic ordering lead to many interesting effects, such as the band-gap reduction, VB splitting and polarization dependence of the optical transitions [6]. The schematic energy-band diagram of the disordered zinc-blende and ordered CuPt-B structures at the G point, where the electronic states are labeled in Slater–Koster notation [7] is shown in Figure 6.3. The essential difference between the potential that an electron experiences in an ideal zinc-blende lattice and that in an ordered CuPt-B structure is the relatively small differences in ‘crystal field (Dscr )’ due to sites beyond the next nearest neighbors. The detailed differences in the energy bands then arise from the difference in the crystal field and also from the SL nature in ordered materials. These can be briefly summarized as follows [6]: 1. The lowest CB G4 in the CuPt-B structure corresponds to the CB G6 in the zinc-blende structure, whereas the upper CB G4 derives from the back-folded L-point CB minimum L6. Because of the same symmetry of these states their energies are shifted compared to those of

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

137

Table 6.2 E0a (a ¼ A, B or C) or related excitonic gap energy for some wurtzite group-IV, III–V and II–VI semiconductors at 300 K System

Material

IV III–V

2H-SiC AlN GaN InN BeO MgSe ZnO ZnS CdS CdSe CdTe

II–VI

a b

E0A (eV)

E0B (eV)

3.330a 6.2 3.420 0.70 10.6 4.1b 3.45 3.75 2.501 1.751 1.56b

E0C (eV)

3.428

3.40 3.78 2.516 1.771

3.55 3.87 2.579 2.176

At 4.2 K Estimated

the ordered Ga0.5In0.5P due to the level repulsion by a certain amount, the value of which increases with increasing order parameter h. This leads to a reduction in the gap between the upper VBs G5, G6 and the lowest CB G4, whereas the gap to the second lowest CB G4(L6) increases. 2. Due to reduction of symmetry with regard to the order direction ½111, the degeneracy of the j ¼ 3/2 states at the G point is lifted. The G5, G6 states correspond to the (3/2, 3/2) HH and the G4 state to the (3/2, 1/2) LH band. The VB splitting between the G5, G6(A) and G4(B) states again increases with increasing order parameter h. The VB SO split-off band G4(C) shows a rather weak dependence on the order parameter for the usual values of h < 0.5.

Disordered (Td) L1

Ordered (C3v)

L6 Γ1

Γ4 Γ6

Γ4 E0

Γ15

E0+∆0

E0A E0B

E0C

Γ8

Γ5, Γ6 (A) Γ4 (B)

∆so=∆0 Γ7

(a) ∆so=∆cr=0

(b) ∆cr=0

Γ4 (C) (c) ∆sso>0, ∆scr>0

Figure 6.3 Schematic energy-band diagram of the disordered zinc-blende and ordered CuPt-B structures at the G point. Note that the upper CB G4 in (c) derives from the back-folded L-point CB minimum L6 in (b)

138

PROPERTIES OF SEMICONDUCTOR ALLOYS

The triply degenerate G15 VB in Figure 6.3(a) is split into three states by the SO (Dsso ¼ Ds0 ) and crystal-field interactions (Dscr ). These three states can be described by the same model as that in Equation (6.1) by replacing Dso with Dsso and Dcr with Dscr . The VB splitting at the top of the VB for CuPt-B ordering can then be given by sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ s Dsso þ Dscr Dso þ Dscr 2 2 s s ð6:3aÞ Dso Dcr DEBA ðhÞ ¼ E0B ðhÞE0A ðhÞ ¼ 3 2 2 Ds þ Dscr þ DECA ðhÞ ¼ E0C ðhÞE0A ðhÞ ¼ so 2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ s Dso þ Dscr 2 2 s s Dso Dcr 3 2

ð6:3bÞ

The quantities that are experimentally accessible are DEBA(h), DECA(h) and Eg(h) ¼ E0A(h) for partially ordered alloys and for random alloys. These values can be used to derive Dsso ðhÞDsso ð0Þ ¼ Dsso ðhÞD0 ¼ h2 ½Dsso ð1ÞD0

ð6:4aÞ

Dscr ðhÞDscr ð0Þ ¼ Dscr ðhÞ ¼ h2 Dscr ð1Þ

ð6:4bÞ

DEg ðhÞ ¼ Eg ðhÞEg ð0Þ ¼ h2 DEg ð1Þ

ð6:4cÞ

where h ¼ 0 and 1 describe perfectly disordered (Dsso ð0Þ ¼ D0 and Dscr ð0Þ ¼ 0) and ordered materials, respectively, and DEg(1) represents the maximum band-gap reduction for perfectly ordered material. However, since perfectly ordered (h ¼ 1) samples are unavailable, and also the degree of the order parameter h of a given sample is not usually determined directly, Dsso ð1Þ, Dscr ð1Þ and DEg(1) cannot be found by this fitting procedure. Only the ratio j¼

DEg ð1Þ Dsso ð1ÞD0

ð6:5aÞ

DEg ð1Þ Dscr ð1Þ

ð6:5bÞ

z¼

can be determined from the measurement of DEBA(h), DECA(h) and Eg(h) ¼ E0A(h). On the other hand, if (Dsso ð1ÞD0 ), Dscr ð1Þ and DEg(1) were known independently (e.g. from theoretical calculation), then experimental values for DEBA(h), DECA(h) and Eg(h) could be used to derive h from the above equations. The maximum band-gap reduction for perfectly ordered Ga0.5In0.5P is reported to be 0.47 eV [8]. Perfectly ordered material has, of course, never been observed. In the most ordered Ga0.5In0.5P structure, the highest order parameter h is 0.6 [9] and the degree of ordering is nonuniform on the local scale. In Figure 6.4 the band-gap energy reduction DEg(h) has been plotted against the squared order parameter h2 for Ga0.5In0.5P. The experimental data are taken from Forrest et al. [10]. It has been established that DEg(h) increases almost linearly with increasing h2. The solid line in Figure 6.4 represents the relationship, DEg(h) ¼ 0.49h2 eV. From Equation (6.4c), the maximum band-gap reduction is found to be DEg(1) ¼ 0.49 eV for perfectly ordered Ga0.5In0.5P.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

139

Figure 6.4 Band-gap energy reduction DEg(h) against squared order parameter h2 for Ga0.5In0.5P. The experimental data are taken from Forrest et al. [10]. The solid line shows the relationship, DEg(h) ¼ 0.49h2 eV

6.2 GROUP-IV SEMICONDUCTOR ALLOY 6.2.1 Binary Alloy (a) CSi The indirect and direct gap energies EgX and E0 for diamond and Si, together with those for 3CSiC (x ¼ 0.5) are shown in Figure 6.5. The experimental data are taken from Table 6.1. The solid lines in Figure 6.5 show the best fit of these data using the parabolic expressions (in eV) EgX ðxÞ ¼ 1:12 þ 0:70x þ 3:68x2

ð6:6Þ

E0 ðxÞ ¼ 4:06 þ 2:12x þ 9:12x2

ð6:7Þ

There is, however, some ambiguity about the band-gap energies and band lineups in CxSi1x/Si heterostructures. The large tensile strain in pseudomorphic CxSi1x layers on Si is expected to strongly affect the band edges (see Section 9.1.2). The higher-lying CPs of supersaturated CxSi1x (x < 0.02) have become the origin of some controversy in the literature. Using ER and SE, Kissinger et al. [11] and Zollner et al. [12] found that the E1 gap in CxSi1x increases linearly with increasing x, as shown in Figure 6.6. The slopes in Figure 6.6 at 300 K give DE1 ¼ 35 meV/at%[C] and DE0 0 ¼ 7 meV=at%½C. On the other hand, Demkov and Sankey [13] argued that the band gaps of free-standing CxSi1x should decrease with increasing x. For strained pseudomorphic alloy, the lower of the two strain-split E1 energies should decrease even more. Additional weak structures in the SE spectra of CxSi1x and CxSiyGe1xx at 2.7 and 3.0 eV were, indeed, observed by Zollner et al. [12] and Lee et al. [14]. These structures were interpreted as previously unidentified optical transitions in the materials due to defects or C-related bands [14]. More recently, Zollner et al. [15] suggested

140

PROPERTIES OF SEMICONDUCTOR ALLOYS 18 15

CxSi1-x

Eg (eV)

E0

3C-SiC

12 9 6

E gX

3 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.5 Energies of the indirect gap EgX and direct gap E0 for diamond and Si at 300 K, together with those for 3C-SiC (x ¼ 0.5). The open circles represent the endpoint elemental data in Table 6.1. The solid lines show the best-fit results of these data using Equations (6.6) and (6.7)

that the new structures are actually interference fringes originating from the reflection of light at the alloy/substrate interface. (b) CGe Figure 6.7 shows the lowest indirect gap energies EgX and EgL versus x for CxGe1x. Kolodzey et al. [16] measured the optical absorption spectra of CxGe1x grown on Si(1 0 0) by MBE. Schrader et al. [17] also carried out optical absorption measurements on CxGe1x/Si deposited by hollow-cathode sputtering. The EgL values obtained from these studies are shown in Figure 6.7 by the open and solid circles. The linearly interpolated E0 and EgX values using

3.6 CxSi1-x

Eg (eV)

3.5 E1

3.4

E0'

3.3 T=80 K 300 K 3.2 0

0.3

0.6 0.9 x (at%)

1.2

1.5

Figure 6.6 Energies of the DE00 and E1 CPs versus x for CxSi1x at 300 K. The experimental data are taken from Kissinger et al. [11] (solid and open triangles) and Zollner et al. [12] (solid and open circles). The slopes shown by the solid lines give DE1 ¼ 35 meV/at%[C] and DE00 ¼ 7 meV=at%½C (at 300 K)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

141

1.5

E0

E gID (eV)

1.2

EgX

0.9

EgL

0.6

CxGe1-x

0.3 0

2

4

6

8

10

12

x (at%)

Figure 6.7 Energies of the lowest indirect gaps EgL and EgX and direct gap E0 versus x for CxGe1x at 300 K. The experimental data are taken from Kolodzey et al. [16] (open circles) and Schrader et al. [17] (solid circle). The solid triangles represent the endpoint elemental data in Table 6.1. The solid lines show the calculated results using data in Table 6.3

the endpoint data in Table 6.1 are shown by the solid lines. Table 6.3 summarizes the three main band-gap energies E0, EgX and EgL for CxGe1x. From these results, we can expect the EgX EgL crossover to occur at x 0.1. Extrapolation gives an EgL value of 7.26 eV for diamond. Table 6.3 Energies for some indirect and direct gaps in CxGe1x at 300 K. LF ¼ linear fit; LI ¼ linear interpolation Band Gap

Expression (eV)

Remark

EgL E0 EgX

0.66 þ 6.60x 0.795 þ 14.505x 0.852 þ 4.648x

LF LI LI

The higher-lying CPs, such as E1, E1 þ D1, E0 0 and E2, for CxGe1x have been determined using SE for x up to 0.03 [18]. These CPs are found to be roughly the same as those which do not contain C. (c) SiGe 1. Relaxed alloy—The binary alloy of Si and Ge provides a continuous series of materials with gradually varying physical properties. The physical properties of SixGe1x grown on Si have been under extensive study stimulated by their potential for use in various device applications. Due to the large lattice mismatch (Da/a 4 %), however, the critical layer thickness for pseudomorphic SixGe1x growth decreases drastically with increasing x [19]. The lattice constant of ‘relaxed,’ or in other words ‘unstrained’ SixGe1x, has been measured and showed to obey Vegard law (Section 1.4.3). The composition dependence of the fundamental absorption edge in SixGe1x was first determined by Braunstein et al. [20] using optical absorption and more recently by Weber

142

PROPERTIES OF SEMICONDUCTOR ALLOYS

and Alonso [21] using PL measurements. Figure 6.8(a) shows the results obtained by Braunstein et al. [20]. The crossing-over of the lowest-lying CB states from the L point to the X point (or D direction) is found at x 0.15. Thus, the conduction electron nature of SixGe1x changes from ‘Ge-like’ to ‘Si-like’ at x 0.15. The solid lines in Figure 6.8(a) represent the results calculated from the data in Table 6.4. 1.2

6 (a)

(E0)

1.1

E2 (Σ)

4

0.9

E gD (eV)

E gID (eV)

1.0

E gX

0.8

0.2

E2 (X)

E1+∆1

E0'

3

E0+∆0

0.4

0.6

0.8

E0

1

SixGe1-x 0

E1

2

E gL

0.7 0.6

E1'

5

(b) 1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

x

Figure 6.8 (a) Energies of the fundamental absorption edges EgL and EgX versus x for relaxed SixGe1x at 300 K. The experimental data are taken from Braunstein et al. [20]. (b) Energies of some CPs versus x for SixGe1x at 300 K. The solid circles in (a) and (b) represent the endpoint elemental data in Table 6.1 and Adachi [1]. The solid lines in (a) and (b) show the calculated results using the data in Table 6.4

The direct gap energies in relaxed SixGe1x have been determined using various measurement techniques, such as SE and ER. Table 6.4 summarizes the lowest direct and Table 6.4 Energies for some indirect and direct gaps in relaxed SixGe1x at 300 K. LI ¼ linear interpolation; QF ¼ quadratic fit Band Gap

Expression (eV)

Remark

EgL E0 EgX E0 þ D0 E1 E1 þ D1 E00 E2(X) E2(S) E10

0.66 þ 1.34x 0.795 þ 3.265x 0.852 0.032x þ 0.300x2 1.08 þ 3.05x 2.108 þ 1.134x þ 0.153x2 2.296 þ 1.070x þ 0.062x2 3.03 þ 0.32x 4.291 0.116x þ 0.084x2 4.406 0.005x þ 0.072x2 5.80 0.48x

LI LI QF LI a a a b b LI

a b

C. Pickering et al., Proc. SPIE 1985, 414 (1993) J. H. Bahng et al., J. Phys.: Condens. Matter 13, 777 (2001)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

143

higher-lying direct gap energies in relaxed SixGe1x alloy. Note that the E2 transitions in Si (and SixGe1x) occur not only along the h110i direction (S) but also near the X point (or D direction). All these CPs, including E0 and E0 þ D0, are plotted against x in Figure 6.8(b). Except for E00 and E2, the band-gap energies in SixGe1x are found to be fairly sensitive to x. 2. Strained alloy—The band structure of pseudomorphical SixGe1x epilayers on Si(100) substrates is drastically altered by the built-in strain or stress. The remarkable effect of the biaxial or uniaxial stress on the band structure is to split the HH (3/2, 3/2) and LH (3/ 2, 1/2) degeneracy at the G point (see Figure 8.1 in Adachi [1]). The biaxial tetragonal distortion can also shift and split the CB edge, for example, the sixfold degenerate CB minima at the X point or along D in bulk Si split into twofold and fourfold minima under [001] compressive strain [1]. The fundamental absorption edge of strained SixGe1x/Si(100) has been investigated by several authors using photocurrent [22] and PL [23,24]. These results are summarized in Figure 6.9. The heavy gray lines show the theoretical results obtained by People [25]. The experimental data agree well with the theoretical values.

1.2

1.1

E gL

E gID (eV)

1.0

E gX

0.9

0.8 HH & LH 0.7 SixGe1-x /Si(100) 0.6 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.9 Energies of the fundamental absorption edges EgL and EgX versus x for strained SixGe1x/Si (100) epilayer. The experimental data are taken from Lang et al. [22] (solid triangles, at 90 K), Dutartre et al. [23] (solid circles, at 90 K) and Liu et al. [24] (at 77 K, open circles). The light solid line shows the low-temperature values of relaxed SixGe1x epilayer. The heavy gray lines show the theoretical results of People [25]

144

PROPERTIES OF SEMICONDUCTOR ALLOYS

SE, ER and PR techniques have been used to determine the CP energies in strained SixGe1x/Si epilayers [26–30]. A decrease in the E1 energy with increasing x, compared with that observed in relaxed SixGe1x samples, has been reported [26,27]. On the other hand, Bahng et al. [29] reported an increase in the E1/(E1 þ D1), DE0 0 and E2 energies with increasing in-built strain in strained Si0.8Ge0.2/Si(1 0 0), where the strain was controlled by depositing different thickness of the Si0.8Ge0.2 epilayers from 35 to 350 nm. In the case of the externally applied uniaxial stress X||[0 0 1], the E1 energy in bulk Si decreased (increased) with increasing X for the light polarization E||X (E?X) used in the SE measurements [31]. Therefore, attention must be paid to analyzing the effects of in-built strain on the electronic energy-band structure of strained materials based on the standard DP theory [1]. 3. External perturbation effect—The temperature dependence of the fundamental absorption edge in relaxed SixGe1x alloy was measured by Braunstein et al. [20]. The experimental data were found to be essentially the same as those for bulk Si and Ge [1]. The temperature dependence of the higher-lying CPs in relaxed and strained SixGe1x has been measured by Humlıcek et al. [32] and Ebner et al. [30], respectively. The relaxed alloy data obtained are: dE1/dT (3 1) 104 eV/K and dE2/dT (2–4) 104 eV/K (x ¼ 0–1.0). All strainedalloy CP data also satisfactorily fitted the phenomenological formulas of Varshni and Vi~ na [1]. The influence of hydrostatic pressure on the ER spectra of relaxed SixGe1x alloy has been reported to be given by dE1/dp ¼ 7.8 1.6x meV/kbar and dE0 0 =dp ¼ 1:40:4x meV=kbar [33]. (d) GeSn The fundamental absorption edge in GexSn1x is expected to change from the Ge L6 indirect to the Sn G7 direct gap depending on x. The band structure near the direct–indirect transition region in relaxed or epitaxial GexSn1x films has been studied using optical absorption [34,35], SE [36,37] and PR [37]. Figure 6.10(a) shows the E0 and EgL energies versus x for nearly relaxed GexSn1x (1.0 > x 0.85) deposited on 10 nm thick relaxed Ge buffer layers on Si(100) substrates by MBE [34] and those obtained for epitaxial GexSn1x films (1.0 > x 0.86) deposited on Ge(100) substrates by rf magnetron sputtering [35]. Note that a-Sn (gray tin) is a zero gap semiconductor (i.e. semimetal) with degenerate valence and conduction bands at the center of the BZ. Thus, the lowest direct gap energy E0 (G8 þ ! G7) in a-Sn has a negative value (0.413 eV at 1.5 K, see Table 6.1). The solid lines in Figure 6.10(a) represent the quadratic fits of the experimental data. The resulting expressions are given in Table 6.5. These expressions predict that E0 and EgL become zero at x 0.67 and 0.25, respectively. GexSn1x should therefore be a semimetal at up to x 0.7. These expressions also predict that E0 and EgL cross at x 0.88. The interband transition energies in GexSn1x have been studied by D’Costa et al. [37]. Because of insufficient sensitivity of SE for energies below 1 eV, they carried out PR measurements at 15 K. Like E0 (Figure 6.10(a)), E0 þ D0, E1/(E1 þ D1), E00 and E2 decreased with increasing Sn concentration. From the quadratic fits of the 15 K data, they determined the bowing parameter of each CP. Introducing these parameters and binary data into Equation (A.17), we obtain the CP energies of GexSn1x at 300 K, as listed in Table 6.5. The numeric results of these expressions are shown in Figure 6.10(b).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

5

0.9

(a)

(b)

4

E0

0.6

E2

E gL E gD (eV)

E0,E gL (eV)

3 0.3 E gL

0

E0 ' E1+∆1

2

E1

1 E0 -0.3

0

0.2

0.4

0.6

0.8

E0+∆0

0

Ge x Sn 1-x -0.6

145

1.0

-1

E0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.10 (a) Energies of the lowest direct E0 (solid circles) and lowest indirect gap EgL (open circles) versus x for GexSn1x at 300 K. The experimental data are taken from He and Atwater [34] and de Guevara et al. [35]. (b) Energies of some CPs versus x for GexSn1x at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.5 Table 6.5 Energies for some indirect and direct gaps in GexSn1x at 300 K. QF ¼ quadratic fit Band Gap E0 EgL E0 þ D0 E1 E1 þ D1 E00 E2 a

Expression (eV) 0.413 0.617x þ 1.826x2 0.092 0.702x þ 1.275x2 0.40 2.36x þ 3.04x2 1.25 0.79x þ 1.65x2 1.65 0.39x þ 1.05x2 2.25 þ 0.25x þ 0.49x2 3.02 þ 0.97x þ 0.40x2

Remark QF QF a a a a a

Bowing parameter is obtained from V. R. D’Costa et al. (Phys. Rev. B 73, 125207 (2006))

6.2.2 Ternary Alloy (a) CSiGe As mentioned in Section 1.4.3, CxSiyGe1xy can be grown lattice-matched on Si substrate. The smaller C addition compensates the compressive strain in SixGe1x binary layers and thus relieves thickness limitations in SixGe1x growth. Furthermore, the major band offset in SixGe1x/Si heterojunction is in the CB, which, in connection with the VB offset in the SixGe1x/Si, has already been opened up a wide variety of new electronic and optical properties within the SixGe1x/Si heterojunction system. Amour et al. [38] have grown pseudomorphic CxSiyGe1xy/Si(100) layers by rapid thermal CVD and measured PL spectra at temperatures between 2 and 77 K. We show in Figure 6.11 the lowest gap energy EgL versus biaxial compressive strain for pseudomorphic SixGe1x (adopted

146

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.2

E Lg (eV)

1.1

pm - Si xGe 1-x z =0.24

1.0 z =0.38 0.9 pm - Cx Si y Ge 1-x-y

0.8

0

0.005

0.010 e bcs

0.015

0.020

Figure 6.11 Energies of the fundamental absorption edge EgL versus biaxial compressive strain ebcs for pseudomorphic (pm-) SixGe1x and pm-CxSiyGe1xy (z ¼ 1xy) at 77 K. The experimental data are taken from Amour et al. [38] (solid and open circles). The pm-SixGe1x line is taken from Van de Walle and Martin [39]. The ebcs ¼ 0 compositions are estimated to be x ¼ 0.05 (0.03) and y ¼ 0.57 (0.73) for z ¼ 0.38 (0.24)

from Van de Walle and Martin [39]) and Amour’s data. Adding C into SixGe1x and keeping the constant Ge content, the strain decreases and EgL increases, but the increase in EgL is much less than it would be if the strain was reduced simply by reducing the Ge content without adding C atoms. Amour et al. considered that for a given band gap, CxSiyGe1xy has less strain than does SixGe1x. The average slope of the CxSiyGe1xy data, DEgL /Debcs ¼ 6.1 eV/unit strain, corresponds to DEgL /Dx ¼ þ 21 meV/at%[C] [38]. Furthermore, by linearly extrapolating the CxSiyGe1xy data to zero ebcs, a significant band offset to Si for strain-free CxSiyGe1xy films is obtained. For z ¼ 1 x y ¼ 0.38, the band offset would be 0.19 eV. From Table 1.8, we can estimate the ebcs ¼ 0 compositions to be x ¼ 0.05 (0.03) and y ¼ 0.57 (0.73) for z ¼ 0.38 (0.24). Schmidt and Eberl [40] grew strained, exactly strain compensated and compressively strained CxSiyGe1xy layers on Si by MBE and measured their PL spectra at 8 K. In Figure 6.12 EgL has been plotted against Ge composition for exactly strain compensated, relaxed CxSiyGe1xy layers obtained by Schmidt and Eberl. Note that the EgL energies plotted in Figure 6.12 were obtained from the zero-phonon PL peaks by adding the indirect-exciton binding energy to coincide with the value of EgL ¼ 1.17 eVat 8 K for bulk Si [1]. These plots can be fitted by a linear decrease with DEgL /Dz ¼ 8.4 meV/at%[Ge], or equivalently, DEgL / Dx ¼ 68 meV/at%[C]. Schmidt and Eberl [40] also observed an initial increase in PL peak energies on the way from tensile strained CxSi1x as well as from compressively strained SixGe1x towards exactly strain compensated CxSiyGe1xy.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

147

1.17 1.16 r - Siy Ge1-x

E Lg (eV)

1.15 1.14 1.13 1.12

sc-Cx Siy Ge1-x-y

1.11

T =8 K

1.10 1.09 0

1

2

3

4 5 Ge (at%)

6

7

8

Figure 6.12 Energies of the fundamental absorption edge EgL versus Ge atomic composition for exactly strain compensated (sc-) CxSiyGe1xy layers at 8 K reported by Schmidt and Eberl [40]. The EgL energies were estimated from the zero-phonon PL peaks by adding the indirect-exciton binding energy to coincide with the band gap of EgL ¼ 1.17 eV at 8 K for bulk Si. For comparison, the relaxed (r-) SiyGe1y line is plotted against Ge atomic composition

The higher-lying CPs, such as E1 and E2, in CxSiyGe1xy/Si(100) films were studied using SE and ER [18,41,42]. The E1 gap increased and the E2 gap decreased as x increased for Si-rich CxSiyGe1xy alloy [41,42]. For Ge-rich CxSiyGe1xy alloy, C had no detectable influence on the higher-lying CPs [18]. (b) SiGeSn Single-phase SixGeySn1xy alloys with x 0.25 and y 0.64 were grown on Si(100) by CVD [43,44]. SE of selected samples yielded dielectric functions indicating a band structure consistent with highly crystalline semiconductors of diamond symmetry. Incorporation of Si into GexSn1x led to an additional reduction of E2, as expected based on the E2 values of Si and Ge [43].

6.2.3 Summary We have discussed the energy band gaps in some group-IV semiconductor alloys. Figure 6.13 summarizes the fundamental absorption gap Eg versus lattice constant a for some binary alloys. We find that all binary gaps, except for GexSn1x (0 x 0.88), are indirect. The GexSn1x alloy for 0.67 x 0.88 is a direct gap semiconductor, but becomes semimetallic for x 0.67. We can thus suppose that almost all ternary gaps, like CxSiyGe1xy, are indirect. CxSi1x is estimated to have an indirect gap at X (EgX ) over the whole composition range, while CxGe1x may have an indirect gap at L (EgL ) for 0 x 0.09 and at X for the rest. The band-gap energy of CxGe1x lattice-matched to 3C-SiC can be derived from Figure 6.13. The lattice constant a of 3C-SiC is 4.3596 A. The corresponding x and EgX for CxGe1x/3C-SiC are 0.62 and 3.7 eV, respectively. The fundamental absorption edge of 3C-SiC is 2.39 eV (EgX , Table 6.1). Because of its wide band-gap nature, C0.62Ge0.38 can be used as a new gate or a

148

PROPERTIES OF SEMICONDUCTOR ALLOYS 6 C 5

Eg (eV)

4 3 3C-SiC

2

Ge

1

Si

α -Sn

0 semimetallic -1 3.5

4.0

4.5

5.0

5.5

6.0

6.5

a (Å)

Figure 6.13 Lowest band-gap energy Eg versus cubic lattice constant a for some group-IV binary alloys at 300 K. The 3C-SiC data is plotted for comparison

barrier material for 3C-SiC FETs. It should be noted, however, that an interpolation scheme proposed by Soref [45] gives the nearly same EgX values between CxGe1x/3C-SiC alloy and 3C-SiC. The E1-gap bowing parameters c are determined to be 0.153 and 1.65 eV for SixGe1x and GexSn1x, respectively (Tables 6.4 and 6.5). In Figure 6.14 these values are plotted against the product DaABDXAB of the lattice constant (DaAB) and electronegativity differences (DXAB) between the elemental semiconductors A and B. The electronegativity values were taken from Phillips’s definition [46]. The bowing parameter c increases almost linearly with increasing product DaABDXAB (c in eV, DaABDXAB in AeV) c ¼ 9:93ðDaAB DXAB Þ

ð6:8Þ

4.0 3.5

E1

3.0

SiSn

c (eV)

2.5 2.0

GeSn

1.5 1.0 0.5 0

SiGe 0

0.1 ∆a ∆X AB

AB

0.2 (Å eV)

0.3

Figure 6.14 Bowing parameter c of the E1 gap versus product DaABDXAB of the lattice-constant and electronegativity differences between the endpoint elements A and B in the binary alloy AxB1x. The SiSn data (open circle) is taken from D’Costa et al. [44]. The solid line represents the calculated result using Equation (6.8)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

149

D’Costa et al. [44] obtained c 3.05 eV for SixSn1x from the SE analyses in the E1/(E1 þ D1) region of SixGeySn1xy. The open circle in Figure 6.14 represents the data of D’Costa et al. We can conclude that the c values in the Si–Ge–Sn alloy system follows a simple scaling behavior that can be expressed in terms of the electronegativity and lattice mismatches (Equation (6.8)). It should be noted, however, that Equation (6.8) estimates in considerably large bowing parameters c for C-related alloys, 20, 24 and 39 eV for CxSi1x, CxGe1x and CxSn1x, respectively. Further study is, therefore, needed to elucidate this unexpected point.

6.3 III–V SEMICONDUCTOR TERNARY ALLOY 6.3.1 (III, III)–N Alloy (a) c-AlGaN Due to their metastable nature, the growth of single-phase cubic nitride films of sufficient homogeneity and crystal quality is still difficult and, in general the crystal quality of the cubic III–N layers grown so far is inferior to that of the hexagonal nitrides. The E0 edge of cAlxGa1xN has been studied using SE [47–49]. These results are shown in Figure 6.15(a). We can see that the experimental data of Kasic et al. [49] gives larger E0 values than those obtained by Suzuki et al. [48]. As a result, the linear interpolation scheme explains Kasic’s data very well, as shown by the heavy solid line. The electronegativity and size mismatch

6 (a) c-AlxGa1-xN

(b) c-GaxIn1-xN

(c) c-AlxIn1-xN

5

E0, E gX (eV)

4 E gX 3

2

c=0 eV c=-1.000 eV E0

1

0 c-AlN

c-GaN

c-InN

c-AlN

x

Figure 6.15 Energies of the lowest direct E0 and indirect gaps EgX for (a) c-AlxGa1xN, (b) c-GaxIn1xN and (c) c-AlxIn1xN at 300 K. The experimental data in (a) are taken from Suzuki et al. [48] (solid circles) and Kasic et al. [49] (open circles) and in (b) from M€ullh€auser et al. [71] (open circle) and Goldhahn et al. [72] (solid circles). The theoretical curves are calculated from Table 6.6

150

PROPERTIES OF SEMICONDUCTOR ALLOYS

product scale also predicts a very small bowing parameter c 0.07 eV for c-AlxGa1xN (Equation (6.23)). No experimental data has been reported on the X- and L-valley gaps EgX and EgL for any binary nitrides or their alloys. All theoretical work, however, has suggested that in all III–N semiconductors the X-valley CB is located at a lower energy than the L-valley CB (i.e. EgX < EgL ) [50]. Thompson et al. [51] carried out SE measurements on c-AlN and concluded from the gradual onset of the absorption edge that c-AlN is an indirect gap semiconductor. The gap that they obtained is 5.34 eV (EgX ). It should be noted, however, that it is very difficult to determine an indirect absorption edge, which usually has very weak transition strength, using SE. Thus, optical absorption or transmission measurements are needed to directly determine whether c-AlN is a direct or an indirect gap semiconductor. The light solid line in Figure 6.15(a) shows the linear interpolation result of the theoretical EgX values for c-AlN and c-GaN [50]. The corresponding EgX and E0 versus x formulas are listed in Table 6.6. The heavy dashed line also represents the result of Equation (A.5) with c ¼ 1.000 eV. This value is recommended for wAlxGa1xN (c ¼ 1.00 eV, see Table 6.7). The E1 and E2 CPs in c-AlxGa1xN are also found to be blue- and red-shifted respectively, with increasing x for x 0.12, [49]. (b) w-AlGaN The experimental E0 versus x data for w-AlxGa1xN [52–55] are shown in Figure 6.16(a). The bowing parameter c of E0 varies widely from upward to deep downward bowing [56,57]. Lee et al. [58] noted that the early findings of an upward bowing have generally not been duplicated. Although there have been many reports of c for x < 0.4, very few data have been reported for

Table 6.6 Energies for some direct and indirect gaps in cubic (III, III)–N tenaries at 300 K. LF ¼ linear fit; LI ¼ linear interpolation; QF ¼ quadratic fit Ternary

Band gap

Expression (eV)

Remark

AlxGa1xN

E0 E0 EgX E0 EgX E0 EgX

3.231 þ 1.969x 3.231 þ 0.969x þ 1.000x2 4.20 þ 1.14x 0.56 þ 4.64x 3.00 þ 2.34x 0.560 þ 2.671x 3.0 þ 1.2x

LF (LI) QF LI LI LI LF (LI) LI

AlxIn1xN GaxIn1xN

Table 6.7 Energy for E0 in some wurtzite (III, III)–N tenaries at 300 K. QF ¼ quadratic Ternary

E0 (eV)

Remark

AlxGa1xN AlxIn1xN GaxIn1xN

3.42 þ 1.78x þ 1.00x2 0.70 þ 1.80x þ 3.70x2 0.700 þ 1.080x þ 1.640x2

QF QF QF

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

151

7 (a) w-AlxGa1-xN

(b) w-GaxIn1-xN

(c) w-AlxIn1-xN

6

E 0 (eV)

5 4 3 2 1 0 c-AlN

c-GaN

c-InN

c-AlN

x

Figure 6.16 Energies of the lowest direct gap E0 for (a) w-AlxGa1xN, (b) w-GaxIn1xN and (c) w-AlxIn1xN at 300 K. The experimental data in (a) are taken from Brunner et al. [52] (solid circles), Muth et al. [53] (open circles), Meyer et al. [54] (solid triangles) and Buchheim et al. [55] (open triangles). The experimental data in (b) and (c) are taken from Wu and Walukiewicz [65] (solid circles), Androulidaki et al. [66] (open circles) and Terashima et al. [67] (solid triangles, (c)). The open squares in (a)–(c) represent the endpoint binary data taken from Table 6.2. The solid lines have been calculated from the data in Table 6.7

x > 0.5 [54,57,59]. It can be seen that such higher x samples tend to give smaller E0 values, although the w-AlN (x ¼ 1.0) value is relatively large (E0 6.2 eV, Figure 6.16(a)). The apparent observation of the stronger bowing in the higher x region is actually an artifact resulting from defect- or impurity-related transitions at energies below the band gap [60]. The solid line in Figure 6.16(a) shows the calculated E0 curve using a recommended value of c ¼ 1.00 eV, as summarized in Table 6.7. This value is in good agreement with the results of Yun et al. [61]. Wethkamp et al. [59] also reported the x dependence of the higher-lying CPs at E1 7 eV and E2 8 eV, together with an unidentified peak at E? 13 eV. The temperature and pressure dependence of the band-gap energies has been measured for III–N binaries [50]. There have, however, been relatively few studies on the III–N alloys. Malikova et al. [62] measured the temperature dependence of the excitonic A, B and C peaks in w-Al0.05Ga0.95N in the 16–434 K range using contactless ER and analyzing the results with Varshni and Bose–Einstein expressions [1]. Brunner et al. [52] measured the absorption spectra of MBE-grown w-AlxGa1xN (0 x 1.0) from 7 K up to room temperature, from which a negligible x dependence of the Varshni coefficients a and b was observed. More recently, Nepal et al. [63] employed deep-UV PL to study the temperature and composition dependence of the band-gap energies of MOCVD-grown w-AlxGa1xN (0 x 1.0) in the range between 10 and 800 K. A quadratic dependence of the Varshni coefficients a and b with x was obtained, from which we can calculate the band-gap energy of w-AlxGa1xN with optional x and T.

152

PROPERTIES OF SEMICONDUCTOR ALLOYS

The pressure dependence of E0 in w-AlxGa1xN at 0 x 0.6 grown by MOCVD on (0001)-sapphire substrates has been investigated by Shan et al. [64] for pressures of up to 9 GPa. They reported dE0/dp to be 40 meV/GPa. (c) c-AlInN No detailed experimental data has been reported on the band-gap energies in c-AlxIn1xN. We, therefore, show in Figure 6.15(c) the linearly interpolated results of E0 and EgX using the experimental and theoretical endpoint data, respectively (Table 6.6). (d) w-AlInN The recent experimental studies which reported the E0 of InN to be appreciably below 1 eV compared to the long-accepted value of 2 eV, have initiated a continuing controversy concerning this fundamental quantity of the least studied III–N binary compound, InN. Also, obtaining high-quality Al-based semiconductors (AlN, AlP, AlAs, etc.) is very difficult as a consequence of its significantly higher contamination with residual impurities. Thus, the standard quadratic expression did not provide a reasonable fit to the compositional variation of E0 in w-AlxIn1xN [56]. The experimental E0 versus x data for w-AlxIn1xN is shown in Figure 6.16(c). The recent literature data are taken from Wu and Walukiewicz [65], Androulidaki et al. [66] and Terashima et al. [67]. These data suggest relatively large downward bowing. The solid line in Figure 6.16(c) shows the parabolic fit of these experimental data. The recommended bowing parameter is very large, c 3.70 eV, as listed in Table 6.7. Goldhahn et al. [68] measured the SE spectra of w-AlxIn1xN at 0 x 0.29 in the energy range up to 9.5 eV and determined the higher-lying CPs E1–E4, together with E0. They increased gradually with increasing x. The bowing parameters c determined for E1 and E2 are 1.8 and 2.7 eV, respectively. The pressure dependence of E0 in w-Al0.25In0.75N has been studied by Li et al. [69]. They also estimated the pressure coefficients for w-AlxIn1xN and expressed them as dE0/dp ¼ 25 þ 20x meV/GPa. (e) c-GaInN The E0 gap in c-InN grown on 3C-SiC(100) has been determined to be 0.56 eV by SE at 300 K [70]. The E0 versus x data for c-GaxIn1xN has also been determined using SE [71,72]. These data together with the linearly interpolated EgX values are shown in Figure 6.15(b). The experimental E0 values are in good agreement with the linearly interpolated E0 result given by the heavy solid line (Table 6.6). (f) w-GaInN The recent crystal growth of high-quality GaxIn1xN epilayers with small x has considerably broadened the composition range over which the bowing could be determined reliably. The E0 versus x data for w-GaxIn1xN are shown in Figure 6.16(b). The data are taken from Wu and Walukiewicz [65] and Androulidaki et al. [66]. A number of larger studies cast doubt on the small bowing parameter in w-GaxIn1xN [56]. For example, the experimental data of Parker et al. [73] implied a bowing of 3.42 eV (4.11 eV) for strained (relaxed) GaxIn1xN epilayers grown on (0001)-sapphire substrates with x < 0.25. However, recent studies of a broad

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

153

compositional range supported the findings of a smaller bowing of 1.4 eV [65,74]. Our recommended bowing parameter in Figure 6.16(b) is 1.640 eV (Table 6.7). Higher-lying CPs have been observed in w-GaxIn1xN using SE [75]. A total of five CPs (A, E1, E2, E3 and E4), together with E0, are observed in the spectral range of 0.5–10 eV. All these CPs showed a weak nonlinearity with x. The E0 gap of w-InN is reported to be 0.70 0.05 eVat 300 K [76]. The Varshni coefficients for w-InN are also reported to be a ¼ 0.41 meV/K and b ¼ 454 K [65]. An up-to-date compilation of various band parameters has been presented in Adachi [1] for group-IV elemental, III–V and II–VI binary semiconductors. By using an interpolation scheme, therefore, it is in principle, possible to estimate the band-gap energies for group-IV, III–V and II–VI semiconductor alloys at any temperature and also any pressure. The temperature dependence of E0 in w-GaxIn1xN has been determined for x ¼ 0.86 [77] and 0.92 [78]. The Varshni coefficients a ¼ 1.0 meV/K and b ¼ 1196 K for x ¼ 0.86 [77] are nearly the same as those for w-GaN (a 1.3 meV/K and b 1200 K) [1]. The pressure dependence of E0 in w-GaxIn1xN with 0.89 x 1.0 grown by MOCVD has been investigated for pressures of up to 9 GPa [78]. The pressure coefficients dE0/dp are 37.5 2.5 meV/GPa (T ¼ 10295 K). The pressure coefficients for samples at 0.5 x 1.0 have also been determined and found to be dE0/dp ¼ 30 5 meV/GPa [69].

6.3.2 (III, III)–P Alloy (a) AlGaP AlxGa1xP has an indirect gap over the whole composition range. Figure 6.17(a) shows the lowest indirect and direct gap energies EgID and E0 as a function of x for AlxGa1xP. The experimental EgX data were obtained from optical absorption measurements [79]. The optical absorption at 6 K measured by Onton et al. [80] provided an indirect gap bowing of c 0.18 eV. More recent CL data obtained at 14 K [81] support a small bowing of 0.13 eV for the lowest indirect gap EgX . However, Figure 6.17(a) shows that good agreement with the experimental data can be achieved by putting c ¼ 0 eV into Equation (A.5). The lowest and higher-lying CPs in AlxGa1xP have been investigated using ER in early studies and SE more recently. The experimental E0 data plotted in Figure 6.17(a) are taken from such studies (Rodrıguez and Armelles [82], Choi et al. [83], etc.). The linear interpolation scheme provides good agreement with the experimental E0 data, as shown by the solid line. The composition dependence of the higher-lying CPs is shown in Figure 6.17(b). The experimental ER and SE data can be satisfactorily fitted by the linear expression against alloy composition x [83]. The corresponding formulas are listed in Table 6.8. Note that the SO split-off energies D0 and D1 are observed to be negligibly small in the III–P semiconductors. From Figure 6.17(b), we can expect crossing ofE00 and E2 at x 0.5, which may be a unique characteristic of this alloy (cf. Figure 6.19). If we simply exchange an assignment of the CPs, namely E00 $ E2, in AlP [83], no such crossing occurs, as demonstrated by the dashed lines in Figure 6.17(b). Note that the E00 and E2 transitions occur at or near the G and X points in the BZ, respectively (Figure 6.1), and that identifying higher-lying CPs is a very difficult task. (b) AlInP AlxIn1xP can be lattice-matched to GaAs at x 0.53. Onton and Chicotka [84] grew bulk AlxIn1xP by a modified Bridgman method and measured the CL spectra at 300 K. The open

154

PROPERTIES OF SEMICONDUCTOR ALLOYS 4.0

6

E2

(a) 5

E0

E0 ' 4

E gL

E gD (eV)

E0,E gID (eV)

3.5

3.0

3

E0 2

E gX

2.5

E1

AlxGa1-xP

1

(b) 2.0 0

0.2

0.4

0.6

0.8

1.0

0 0

x

0.2

0.4

0.6

0.8

1.0

x

Figure 6.17 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxGa1xP at 300 K. The experimental data for E0 are taken from Rodrıguez and Armelles [82], Choi et al. [83], etc., and for EgX from Sonomura et al. [79]. (b) Energies of some CPs versus x for AlxGa1xP at 300 K. The solid lines in (a) and (b) show the calculated results sing the data in Table 6.8. The dashed lines were also obtained by exchanging the E00 $ E2 CP assignment in AlP

Table 6.8 Energies for some indirect and direct gaps in AlxGa1xP at 300 K. LF ¼ linear fit; LI ¼ linear interpolation Band gap

Expression (eV)

Remark

EgX EgL E0 E1 E0 0 E2

2.261 þ 0.219x 2.63 þ 0.94x 2.76 þ 1.15x 3.71 þ 0.59x 4.74 þ 0.40x 5.28 0.65x

LF LI LF LF LF LF

circles in Figure 6.18(a) show these results. A G–X crossing is found to occur at x 0.45. Bour et al. [85] also grew a series of AlxIn1xP on GaAs (100) by MOCVD and determined the E0 energies by ER. These results are also shown in Figure 6.18(a) by the solid circles. The quadratic fit of E0 gives a value of c 0.40 eV, as listed in Table 6.9. No experimental data relating to the higher-lying CPs in AlxIn1xP has been reported. We, therefore, show in Figure 8.18(b) the CP energies obtained from the linear interpolation scheme between the InP (x ¼ 0) and AlP (x ¼ 1.0) data in Adachi [1]. As in Figure 6.17(b) (AlxGa1xP), crossing of E00 and E2 occurs at x 0.4 in AlxIn1xP. This crossing can be removed by simply exchanging the assignment of the CPs, E00 $ E2 , in AlP [83], as demonstrated by the dashed lines in Figure 8.18(b). The electron-HH and electron-LH transition energies in strained AlxIn1xP layers grown on GaAs by MOCVD were investigated at 20 K using a PR technique [86]. The E0 versus x data

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

6

4.0

E2

(a)

5

3.0

E0 '

4

E gL

E gD (eV)

E0, E gID (eV)

3.5

2.5 E gX

3

E1

2

2.0

E0

E0

1.5 1.0

155

1

Al xIn 1-xP 0

0.2

0.4

0.6

0.8

1.0

0

0

(b) 0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.18 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxIn1xP at 300 K. The experimental data are taken from Onton and Chicotka [84] (open circles) and Bour et al. [85] (solid circles). (b) Energies of some CPs versus x for AlxIn1xP at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.9. The dashed lines are also obtained by exchanging the E00 $ E2 CP assignment in AlP Table 6.9 Energies for some direct and indirect gaps in AlxIn1xP at 300 K. QF ¼ quadratic fit; LI ¼ linear interpolation; LF ¼ linear fit Band gap

Expression (eV)

Remark

E0 EgL EgX E1 E00 E2

1.35 þ 2.16x þ 0.40x2 2.05 þ 1.52x 2.21 þ 0.27x 3.71 þ 1.13x 4.70 þ 0.44x 5.10 0.47x

QF LI LF LI LI LI

were also measured for relaxed AlxIn1xP at 20 K [86] and can be expressed as (in eV) E0 ðxÞ ¼ 1:418 þ 2:4x

ð6:9Þ

(c) GaInP GaxIn1xP exhibits some of the largest direct gaps among the non-nitride III–V semiconductors and can be grown lattice-matched to GaAs at x 0.52. This alloy is widely used as a material for various optoelectronic and electronic devices. The lowest direct gap E0 versus x for GaxIn1xP is shown graphically in Figure 6.19(a). The experimental data are taken from Onton et al. [87] (open circles) and Alibert et al. [88] (solid circles). The solid line represents the calculated E0 versus x curve by putting c ¼ 0.65 eV into Equation (A.5). This value is the same as that recommend in Vurgaftman et al. [89]. The G–X crossover is believed to occur at x 0.7 in GaxIn1xP. The indirect band-gap energies EgX for x 0.7 are plotted against x in Figure 6.19(a) by the open triangles. They are

156

PROPERTIES OF SEMICONDUCTOR ALLOYS 3.0

6

E2

(a) 5

E0 '

2.5

E gX

E gL

2.0

E gD (eV)

E0,E gID (eV)

4

0

0.2

0.4

0.6

0.8

E0+∆0

E0

1

Gax In1-x P 1.0

E1

3 2

E0

1.5

E1+∆1

1.0

0 0

(b) 0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.19 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaxIn1xP at 300 K. The experimental data for E0 are taken from Onton et al. [87] (open circles) and Alibert et al. [88] (solid circle) and for EgX from Alibert et al. [88], Lange et al. [90], etc. (open triangles). (b) Energies of some CPs versus x for GaxIn1xP at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.10

taken from Alibert et al. [88], Lange et al. [90], etc. The solid lines represent the calculated EgX and EgL curves using c ¼ 0.200 and 0.34 eV, respectively. Early theoretical and experimental bowing parameters are summarized by Bugajski et al. [91] and more recent values by Vurgaftman et al. [89]. These results vary widely: c ¼ 0.39–1.36, 0–0.40 and 0.23–0.86 eV for E0, EgX and EgL , respectively. Clearly, the c ¼ 1.03 eV value for EgL recommended by Vurgaftman et al. [89] is out of the reported range of 0.23–0.86 eV. If we assume here that c ¼ 0.34 eV for EgL, which is exactly the same as Hill’s value [92], the c ¼ 0.200 eV value for E0 is also the same as that recommended by Vurgaftman et al. [89] (c ¼ 0.20 eV). The expressions for such energy gaps are summarized in Table 6.10. Table 6.10 Energies for some direct and indirect gaps in GaxIn1xP at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

1.35 þ 0.76x þ 0.65x2 1.46 þ 0.73x þ 0.65x2 2.05 þ 0.24x þ 0.34x2 2.210 0.149x þ 0.200x2 3.17 0.32x þ 0.86x2 3.29 0.33x þ 0.86x2 4.70 þ 0.04x 5.10 þ 0.18x

a a b b c c LI LI

Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) Bowing parameter is obtained from R. Hill (J. Phys. C: Solid State Phys. 7, 516 (1974)) c Bowing parameter is obtained from C. Alibert et al. (Phys. Rev. B 6, 1301 (1972)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

157

The composition dependence of the higher-lying CPs for GaxIn1xP has been investigated using ER [88] and SE [93]. These studies observed remarkable bowing (c 0.9 eV) for the E1 and E1 þ D1 transitions. The GaxIn1xP samples used by Lee et al. [93] were epitaxially grown on GaAs and graded-GaInP/GaP substrates by various techniques, such as MOCVD, gassource MBE, LPE or HT-VPE. They mainly investigated the strain and disorder effects of the electrical and optical properties. The general behavior of the E1/(E1 þ D1) peak shifts was explained in terms of the biaxial strain and strain relaxation caused by lattice mismatch. The solid lines in Figure 6.19(b) show the results calculated from Table 6.10. Since the SO split-off energies D0 and D1 are mainly characterized by the nature of the anion atom, the common anion alloys like GaxIn1xP and ZnxCd1xTe have nearly the same D0 or D1 energies, irrespective of alloy composition x. Therefore, in such alloys the E0 þ D0 and E1 þ D1 gaps have nearly the same bowing parameters as the E0 and E1 gaps, respectively. The temperature dependence of the fundamental absorption edge of GaxIn1xP (x ¼ 0–1.0) has been investigated from 20 to 300 K by Ishitani et al. [94]. The same studies, but using samples lattice-matched to GaAs (x 0.5), have also been carried out using PzR [95] and SE [96]. The measured data were analyzed using some empirical expressions, such as Varshni and Bose–Einstein formulas. Onton and Chicotka [97] also undertook PL measurements on GaxIn1xP at 2 K and obtained the x-dependent E0 and EgX values given by (in eV) E0 ðxÞ ¼ 1:409 þ 0:695x þ 0:758x2

ð6:10Þ

EgX ðxÞ ¼ 2:321 þ 0:017x

ð6:11Þ

The pressure dependence of the fundamental absorption edge of GaxIn1xP has been determined by several authors [98,99]. The pressure coefficients dE0/dp and dEgX /dp reported by Hakki et al. [98] were 125 5 meV/GPa (x 0.5) and 11.5 1.5 meV/GPa (x ¼ 0–1.0), respectively. Go~ ni et al. [99] found from optical absorption studies that G–X crossing occurred at 5.0 GPa for x ¼ 0.36 and at 2.7 GPa for x ¼ 0.5 at 300 K. PL measurements were also carried out to investigate G–X crossing as a function of pressure for GaxIn1xP epilayers grown on GaAs(100) substrates [100,101].

6.3.3 (III, III)–As Alloy (a) AlGaAs AlxGa1xAs is known to be the most important and the most investigated III–V semiconductor alloy. Figure 6.20(a) shows the lowest direct and indirect gaps E0, EgL and EgX versus x for AlxGa1xAs. Theexperimentaldatafor E0 aretakenfromAubel etal. [102] and Aspnes etal.[103], for EgL from Saxena [104] and for EgX from Monemaret al. [105].The solid lines are calculated from the data in Table 6.11. The expression for E0 is determined from the SE analysis [103]. This expression reveals that the bowing parameter is x-dependent in the manner (in eV) shown below E0 ðxÞ ¼ ¼

1:430 þ 1:707x1:437x2 þ 1:310x3 1:430 þ 1:580x þ xð1xÞð0:1271:310xÞ

ð6:12Þ

Using Equation (6.12), we can obtain good agreement with the experimental results. It should be noted, however, that almost all AlxGa1xAs data have been explained by the quadratic expression with c ranging from 0.25 to þ 1.147 eV [106].

158

PROPERTIES OF SEMICONDUCTOR ALLOYS

6 3.0

(a)

2.5

E gX

2.0

E0 '

4

E gL E gD (eV)

E0, E gID (eV)

E2

5

E1+∆1 E1

3 E0+∆0

E0

2 E0

1.5

1

Alx Ga1-x As 1.0

0

0.2

0.4

0.6

0.8

1.0

x

0

0

(b) 0.2

0.4

0.6

0.8

1.0

x

Figure 6.20 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxGa1xAs at 300 K. The experimental data for E0 are taken from Aubel et al. [102] and Aspnes et al. [103] (open circles), for EgL from Saxena [104] (solid circles) and for EgX from Monemar et al. [105] (solid triangles). (b) Energies of some CPs versus x for AlxGa1xAs at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.11. The dashed line in (b) also represents the result calculated using Equation (6.13)

Many reports support the hypothesis that the c value for EgL is almost equal to zero. Lee et al. [107], however, reported a value of c ¼ 0.055 eV from PL measurements. The plots produced by Saxena [104] also suggested c ¼ 0 eV for EgL, independent of temperature [108]. As seen from Figure 6.20(a), GaAs is a direct gap semiconductor with G–L–X valley ordering, while AlAs is an indirect gap semiconductor with exactly the reverse ordering. The G–X crossover composition xc for AlxGa1xAs was determined at various temperatures [106] and found to be 0.4 at 300 K and 0.38 at low temperatures. The higher-lying CPs in AlxGa1xAs have been determined by many authors [106]. The bowing parameter of c 0.39 eV was reported for E1, while the E2 gap showed an almost liner variation with x. Such results are shown in Figure 6.20(b) (see also Table 6.11). Aspnes Table 6.11 Energies for some direct and indirect gaps in AlxGa1xAs at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

1.430 þ 1.707x 1.437x2 þ 1.310x3 1.72 þ 0.65x 1.760 þ 1.053x þ 0.407x2 1.910 þ 0.185x þ 0.055x2 2.890 þ 0.518x þ 0.392x2 3.130 þ 0.479x þ 0.391x2 4.52 þ 0.10x 5.13 0.26x

a LI b c b b LI LI

Bowing parameter is obtained from D. E. Aspnes et al. (J. Appl. Phys. 60, 754 (1986)) Bowing parameter is obtained from J. L. Aubel et al. (J. Appl. Phys. 58, 495 (1985)) c Bowing parameter is obtained from H. J. Lee et al. (Phys. Rev. B 21, 659 (1980)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

159

et al. [103] reported an expression analogous to Equation (6.12) for E1 (in eV) E1 ðxÞ ¼ 2:924 þ 0:965x þ xð1xÞð0:1570:935xÞ

ð6:13Þ

The dashed line in Figure 6.20(b) represents the calculated result of this expression. Traditionally, temperature variation of the band-gap energy Eg is expressed in terms of the Varshni formula [1] Eg ðTÞ ¼ Eg ð0Þ

aT 2 T þb

ð6:14Þ

where Eg(0) is the band-gap energy at 0 K, a is in electron volts per Kelvin and b is closely related to the Debye temperature of the material (in Kelvin). The E0-gap Varshni parameters E0(0), a and b for AlxGa1xAs are shown in Figure 6.21(a). The experimental data were 15

β (K)

2.5

(a)

(b)

2.0

12

1.5 11 10 9 8 7 6 5 4 350 300 250 200 150

dE0/dp (10-2eV/GPa)

α (eV/K)

E0(0) (eV)

3.0

9

6 AlxGa1-xAs

3

0

0.2

0.4

0.6 x

0.8

1.0

0 0

0.2

0.4

0.6

0.8

1

x

Figure 6.21 (a) Varshni parameters Eg(0), a and b versus x for E0 in AlxGa1xAs. The solid lines represent the liner least-squares fits summarized in Table 6.12. (b) Pressure coefficient dE0/dp versus x for AlxGa1xAs. The experimental data are taken from Adachi [106]. The solid line shows the calculated result using Equation (6.15)

gathered from various sources. The solid lines represent the linear least-squares fits summarized in Table 6.12. The Varshni parameters for EgL and EgX are also listed in Table 6.12. Introducing such parameters into Equation (6.14), we obtain the E0, EgL and EgX energies for optional alloy compositions (0 x 1.0) and T from 0 up to at least 400 K. The Varshni parameters for the higher-lying CPs were reported in Adachi [106]. There is some considerable variation in the absolute pressure coefficients of E0 and they are limited to x 0.5 [106]. However, the literature data in Figure 6.21(b) can probably be best summarized by (in 102 eV/GPa) dE0 ðxÞ ¼ 11:61:1x ð6:15Þ dp

160

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.12 Varshni parameters defined by Equation (6.14) for E0, EgL and EgX in AlxGa1xAs Band gap

Eg(0) (eV)

a (104 eV/K)

b (K)

E0a EgL b EgX b

1.513 þ 1.380x 1.775 þ 0.792x 1.988 þ 0.207x þ 0.055x2

5.8 þ 3.6x 6.1 4.6–1.0x

206 þ 123x 204 204

Obtained from Figure 6.21 S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties. World Scientific, Singapore, 1994 a b

The EgL and EgX data showed no clear x-dependent pressure coefficients that can be approximated as dEgL =dp 5:5 102 eV=GPa and dEgX =dp 1:5 102 eV=GPa [106]. The pressure coefficients of E1 and E1 þ D1 were approximated as (78) 102 eV/ GPa [106]. (b) AlInAs AlxIn1xAs can be grown lattice-matched to InP at x 0.48 and serve as a barrier layer in the important Ga0.47In0.53As/Al0.48Ga0.52As/InP heterostructure system. Wakefield et al. [109] undertook CL measurements on AlxIn1xAs/InP(100) at x 0.5 and obtained a value of c ¼ 0.74 eV for E0. More recently, Chou et al. [110] determined c 0 eV from PR in the limited composition range 0.43 x 0.58. The experimental data of Chou et al. (solid circles) are shown in Figure 6.22(a). The E0 energy for Al0.48In0.52As/InP was reported to be 1.439 0.005 eV at 300 K [111]. The open circle in Figure 6.22(a) shows this data. From these data, we obtain a value of c 0.72 eV, in good agreement with the earlier work of Wakefield et al. [109].

6

3.5

(a)

3.0

E0 '

4

2.0

E gD (eV)

E0,E gID (eV)

2.5 E gX

1.5 E gL

1.0

0.2

E1 E0+∆0

2

0.4

0.6 x

0.8

E0

1

Alx In1-x As 0

E1+∆1 3

E0

0.5 0

E2

5

(b) 1.0

0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.22 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxIn1xAs at 300 K. The experimental data are taken from Chou et al. [110] (solid circles) and Oertel et al. [111] (open circle). (b) Energies of some CPs versus x for AlxIn1xAs at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.13

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

161

The linear interpolation scheme, used to estimate the L- and X-valley minima, also implies G–X crossover occurring at x 0.63 in Figure 6.22(a). The higher-lying CPs in AlxIn1xAs have been studied using SE [82] and normal-incidence reflectivity [112]. These studies determined the E1-gap c value to be 0.86 and 0.38 eV, respectively. Avalue of c ¼ 0.39 eV was also determined for E1 þ D1 [112]. The recommended band-gap expressions for AlxIn1xAs are summarized in Table 6.13. Table 6.13 Energies for some direct and indirect gaps in AlxIn1xAs at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

0.359 þ 1.931x þ 0.720x2 0.726 þ 1.774x þ 0.720x2 1.07 þ 1.30x 1.37 þ 0.78x 2.50 þ 0.92x þ 0.38x2 2.78 þ 0.83x þ 0.39x2 4.44 þ 0.18x 4.70 þ 0.17x

a b LI LI c c LI LI

Obtained from Figure 6.22 Postulated bowing parameter equal to that for E0 c Bowing parameter is obtained from A. Convertino et al. (J. Vac. Sci. Technol. B 20, 248 (2002))

a b

(c) GaInAs GaxIn1xAs remains a direct gap material over the whole composition range. We show in Figure 6.23(a) the lowest direct and indirect gaps E0, EgL and EgX versus x for GaxIn1xAs. The E0 versus x data are taken from Nahory et al. [113] (open circles) and Kim et al. [114] (solid circles). Ga0.47In0.53As/InP has an energy E0 ¼ 0.728 0.002 eV at 300 K [115]. The open triangle in Figure 6.22(a) shows this value. From these data points, we obtain a value of c 0.58 eV for E0, slightly larger than that recommended by Vurgaftman et al. [89] (c ¼ 0.477 eV). Singh [116] reviewed the E0 gap in lattice-matched and strained Ga0.47aIn0.53 þ aAs grown on InP(100). He obtained the following expression for unstrained samples with small a at 300 K (in eV) E0 ðaÞ ¼ 0:751:05a þ 0:45a2

ð6:16Þ

with zero HH–LH splitting, while for strained samples (in eV) E0 ðaÞ ¼ 0:750:63a þ 0:45a2

ð6:17Þ

with HH–LH splitting of 0.42a eV. There is no reliable experimental technique to determine the L- and X-valley gaps EgL and EgX in GaxIn1xAs. The c values in Table 6.14 are assumed to have a composite value in the range compiled by Vurgaftman et al. [89]. The dashed lines in Figure 6.22(a) represent the EgL and EgX values calculated using Vurgaftman’s recommended c values.

162

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.0

6

(a)

(b)

E2

5 E gX

E0 '

4 1.0

E gD (eV)

E0, E gID (eV)

1.5

E gL

E0

E1+∆1

3

E1

2

E0+∆0

0.5 1

Gax In1-x As 0 0

0.2

0.4

0.6

0.8

E0 1.0

x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.23 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaxIn1xAs at 300 K. (b) Energies of some CPs versus x for GaxIn1xAs at 300 K. The experimental data in (a) and (b) are taken from Nahory et al. [113] (open circles), Kim et al. [114] (solid circles) and Gaskill [115] (open triangle). The solid lines in (a) and (b) show the calculated results using the data in Table 6.14. The dashed lines in (a) are calculated using c ¼ 0.33 and 1.4 eV for EgL and EgX , respectively

The higher-lying CPs in GaxIn1xAs have been determined using SE [114]. These results are shown in Figure 6.23(b). The samples were grown on InP(100) at a thickness of 1 mm, which exceeds the critical thicknesses of strain relaxation. Thus, the data presented in Figure 6.23 represent those for bulk materials. Andreani et al. [117] used PR and SE to investigate the optical response and energy-band structure of a series of strained and relaxed GaxIn1xAs (x > 0.85) films on GaAs(100) substrates. They observed that the energy shifts in E1 and E1 þ D1 due to built-in strain were in good agreement with those calculated from standard DP theory. The solid lines in Figure 6.23(b) were obtained by the analysis of Kim’s data [114] or using the linear interpolation scheme. These results are summarized in Table 6.14. Table 6.14 Energies for some direct and indirect gaps in GaxIn1xAs at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

0.359 þ 0.491x þ 0.580x2 0.726 þ 0.454x þ 0.580x2 1.07 þ 0.15x þ 0.50x2 1.37 0.16x þ 0.70x2 2.50 0.16x þ 0.55x2 2.78 þ 0.03x þ 0.32x2 4.44 þ 0.08x 4.70 þ 0.43x

a b c c d d d LI

Obtained from Figure 6.23 Postulated bowing parameter equal to that for E0 c Estimated from list by I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) d Estimated from data by T. Y. Kim et al. (Phys. Rev. B 68, 115323 (2003)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

163

2.0

E0(0) (eV)

1.5

GaxIn1-xAs

1.0 (a)

0.5 0

α (eV/K)

6 5 4 (b)

3 2 500 β (K)

400

(c)

300 200 100 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.24 Varshni parameters Eg(0), a and b versus x for E0 in GaxIn1xAs. The solid lines represent the liner least-squares fits of Equation (6.18)

The Varshni parameters E0(0), a and b for E0 in GaxIn1xAs are plotted in Figure 6.24. The experimental data have been gathered from various sources (e.g. Hang et al. [118]). The solid lines show the liner least-squares fits given by E0 ð0ÞðxÞ ¼ 0:359 þ 1:154x eV

ð6:18aÞ

aðxÞ ¼ ð3:3 þ 2:5xÞ 104 eV=K

ð6:18bÞ

bðxÞ ¼ 21711x K

ð6:18cÞ

No detailed pressure dependence of the band-gap energies in GaxIn1xAs has been reported. It should be noted, however, that the pressure dependence for GaAs and InAs can be given by dE0/dp ¼ 107 and 114 meV/GPa [1], respectively. Thus, we suggest the value of dE0/dp for GaxIn1xAs to be 110 meV/GPa, independent of x.

6.3.4 (III, III)–Sb Alloy (a) AlGaSb The bowing parameter c for E0 in AlxGa1xSb was determined using various techniques, such as PL, optical absorption and ER [119–121]. The reported c values varied widely from 1.18

164

PROPERTIES OF SEMICONDUCTOR ALLOYS

to þ 0.69 eV [89]. Alibert et al. [119] obtained c ¼ 0.47 and 0.48 eV at room temperature and low temperatures, respectively, and made a detailed comparison between these and previous results. More recently, Bignazzi et al. [120] obtained a better fit to the optical absorption data assuming a linear band-gap variation at low x. These results were confirmed by Bellani et al. [121] from TR measurements at T ¼ 90–300 K. Consequently, a cubic expression was proposed for E0 in AlxGa1xSb E0 ðxÞ ¼ 0:723 þ 1:547x þ ð0:0441:220xÞxð1xÞ ¼ 0:723 þ 1:591x1:264x2 þ 1:220x3

ð6:19Þ

The calculated result of this expression is shown in Figure 6.25(a), together with the experimental data [119,121]. The experimental data in the higher x region in Figure 6.25(a) suggest that the X-valley gap EgX has no strong composition dependence. The experimental G–L crossover composition also suggests that the bowing parameter may be negligibly small for EgL [89]. 5

2.5 Alx Ga1-x Sb

E2 4

2.0

E0 '

1.5

E gD (eV)

E0,E gID (eV)

E gL E gX

E0

1.0

3

E1 2

1

0.5

(a) 0

0

0.2

0.4

0.6 x

0.8

E1+∆1

E0+∆0 E0 (b)

1.0

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.25 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxGa1xSb at 300 K. The experimental data are taken from Anderson et al. (see Alibert et al. [119]) (open circles) and Bellani et al. [121] (solid circles). The solid line (E0) shows the calculated result using Equation (6.19). (b) Energies of some CPs versus x for AlxGa1xSb at 300 K. The solid lines in (a) and (b) show the calculated results using the data in Table 6.15

The higher-lying CPs in AlxGa1xSb have been studied using modulation spectroscopy, such as PzR and ER [119,122] and SE [123,124]. The bowing parameters obtained from these studies are in the range 0.28–0.63 eV. Since the data of Choi et al. were limited to 0 x 0.39 [124], they were fitted using a linear expression. The recommended band-gap expressions for AlxGa1xSb are summarized in Table 6.15. The linear temperature coefficient dE0/dT was reported to be 4 104 eV/K for 0 x 1.0 [121] and x 0.4 [122]. The linear temperature coefficient dEgX =dT was also reported to be (3.1 0.2) 104 eV/K for x > 0.52 [119]. The Varshni parameters E0(0), a and b have been determined for x ¼ 0.12 and 0.19 [125]. However, pressure studies have not been carried out on AlxGa1xSb.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

165

Table 6.15 Energies for some direct and indirect gaps in AlxGa1xSb at 300 K. LI ¼ linear interpolation; LF ¼ linear fit Band gap

Expression (eV)

Remark

E0 EgL EgX E0 þ D0 E1 E1 þ D1 E00 E2

0.723 þ 1.591x 1.264x2 þ 1.220x3 0.760 þ 1.451x 1.050 þ 0.565x 1.50 þ 1.04x þ 0.40x2 2.05 þ 0.49x þ 0.30x2 2.50 þ 0.43x þ 0.30x2 3.56 þ 0.20x 4.14 þ 0.09x

a LI LF b c c LI LI

Bowing parameter is obtained from V. Bellani et al. (Phys. Rev. B 59, 12272 (1999)) Estimated from E0 data c Estimated from various data a b

(b) AlInSb Very limited data are available for AlxIn1xSb [126–128]. Isomura et al. [126] recorded the ER spectra for AlxIn1xSb at 0 x 1.0. They determined the E0, E0 þ D0, E1 and E1 þ D1 energies versus x at 300 K and their results are shown in Figure 6.26, together with those for EgL, EgX , E00 and E2 estimated from the linear interpolation scheme. The corresponding band-gap expressions are listed in Table 6.16. The data in Figure 6.26(a) suggest that AlxIn1xSb is a direct gap semiconductor at x 0.7.

2.5

5 Alx In1-x Sb

E2

2.0

4

E0 '

1.5

E gD (eV)

E0, E gID (eV)

E gX E gL

1.0

3

2

E1+∆1 E1

E0 0.5

1

E0

(a) 0 0

0.2

0.4

0.6 x

0.8

E0+∆0

1.0

0 0

(b)

0.2 0.4 0.6 0.8 1.0 x

Figure 6.26 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for AlxIn1xSb at 300 K. The experimental data are taken from Isomura et al. [126] (solid circles). (b) Energies of some CPs versus x for AlxIn1xSb at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.16

166

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.16 Energies for some direct and indirect gaps in AlxIn1xSb at 300 K. LI ¼ linear interpolation Band gap

Expression (eV)

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.17 þ 1.67x þ 0.930 þ 1.281x 1.04 þ 1.16x þ 1.630 0.015x 1.80 þ 0.70x þ 2.30 þ 0.72x þ 3.26 þ 0.50x 3.90 þ 0.33x

a

Remark 0.43x2 0.74x2 0.34x2 0.21x2

a LI a LI a a LI LI

Bowing parameter is estimated from data in S. Isomura et al. (Phys. Status Solidi B 65, 213 (1974))

The bowing parameters obtained from Isomura et al. [126] are 0.34 and 0.21 eV for E1 and E1 þ D1, respectively, while those obtained by Yaozhou et al. [127] are about a factor of 2 larger and are 0.752 and 0.723 eV for E1 and E1 þ D1, respectively. The fundamental absorption edges in AlxIn1xSb layers (0 x 0.25) grown on GaAs substrates were studied by Dai et al. [128] using transmission spectroscopy from cryogenic to room temperature. A linear change of E0 with lattice constant a (or x) was obtained. (c) GaInSb GaxIn1xSb remains a direct gap semiconductor over 0 x 1.0. The bowing parameters c for E0 previously reported are c ¼ 0.413 0.43 eV for bulk samples [129–131] and 0.35 eV for epilayers [132]. A more recent study of a GaxIn1xSb/GaSb(100) epilayer reports c ¼ 0.406 0.009 eV [133], which is in much better agreement with the bulk results. The solid circles in Figure 6.27(a) show the PzR results obtained by Auvergne et al. [130], which give an E0 bowing of 0.415 eV. The considerable uncertainty for the indirect gaps in GaSb (x ¼ 0) and especially InSb (x ¼ 1.0) translates into a poor understanding of the L- and X-valley gap bowing. The c values of 0.40 and 0.33 eV for EgL and EgX in Table 6.17 are taken from Vurgaftman et al. [89]. The higher-lying CPs, E1, E1 þ D1, E00 and E2, in GaxIn1xSb have been studied using ER [129] and SE [134]. The bowing parameters determined from these studies are in reasonable agreement and are shown in Table 6.17 and Figure 6.27(b). The linear temperature coefficient dE0/dT obtained from PzR measurements [130] can be written as (2.75 1.05x) 104 eV/K. Therefore, the linear interpolation scheme can be safely used to obtain the temperature-dependent and may also be used to estimate the pressuredependent band-gap energies in GaxIn1xSb. The necessary binary data are compiled from Adachi [1].

6.3.5 Dilute-nitride III–(V, V) Alloy (a) General Considerations Dilute-nitride III–V alloys, such as GaNxAs1x and GaInNxAs1x, represent a new class of highly mismatched material systems, which have recently attracted great attention [135]. The ‘dilute’ nitrides now mean that a small N fraction of the order of a few percent can be added to a

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS 2.0

5

(a)

(b)

GaxIn1-xSb

E2

4

1.5 E gX 1.0 E gL 0.5

E gD (eV)

E0,E gID (eV)

167

E0

E0 '

3

E1+∆1 2

E1 E0+∆0

1

E0 0

0

0.2 0.4 0.6 0.8 1.0

0

0

0.2 0.4 0.6 0.8 1.0

x

x

Figure 6.27 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaxIn1xSb at 300 K. The experimental data are taken from Auvergne et al. [130] (solid circles). (b) Energies of some CPs versus x for GaxIn1xSb at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.17

conventional non-nitride semiconductor, such as GaAs or GaInAs. Due to large differences in the lattice constant and ionicity between the host binary and N-related binary (Table 6.18), the dilute nitrides exhibit many unusual and fascinating physical properties. Among them the most prominent feature is the giant bowing in the band-gap energy. It is known that a single bowing parameter is inadequate even if the goal is only to describe the band-gap energy for a relatively wide range of compositions. For example, the bowing parameter c for E0 in GaNxAs1x reached 40 eV for a very low N incorporation (x 0.1 at%), and strongly decreased with increasing N fraction [136]. Because of this, we do not recommend that the type of bowing parameter c be used to describe the dilute nitrides [56].

Table 6.17 Energies for some direct and indirect gaps in GaxIn1xSb at 300 K Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.170 þ 0.135x þ 0.415x2 0.93 0.57x þ 0.40x2 1.040 þ 0.045x þ 0.415x2 1.63 0.91x þ 0.33x2 1.80 0.13x þ 0.38x2 2.30 0.08x þ 0.28x2 3.26 þ 0.30x 3.90 þ 0.24x2

a b c b d d d d

Bowing parameter is obtained from D. Auvergne et al. (J. Phys. Chem. Solids 35, 133 (1974)) Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) c Postulated bowing parameter equal to that for E0 d Bowing parameter is obtained from S. M. Vishnubhatla et al. (Can. J. Phys. 47, 1661 (1969)) a b

168

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.18 Lattice mismatch Da/a and Phillips ionicity difference Dfi for some III–(V, V) and (III, III)–V ternaries. Note that III–(N, V) ternaries exhibit ‘strongly perturbed’ characteristics Alloya

|Da|/a (%)

|Dfi|

Alloy b

|Da|/a (%)

|Dfi|

Al(N, P) Al(N, As) Al(N, Sb) Ga(N, P) Ga(N, As) Ga(N, Sb) In(N, P) In(N, As) In(N, Sb)

19.8 22.6 28.6 17.1 20.0 34.9 15.0 21.5 23.0

0.142 0.175 0.199 0.173 0.190 0.239 0.157 0.221 0.257

(Al, Ga)P (Al, Ga)As (Al, Ga)Sb (Ga, In)P (Ga, In)As (Ga, In)Sb Ga(P, As) Ga(P, Sb) Ga(As, Sb) In(P, As) In(P, Sb) In(As, Sb)

0.2 0.1 0.6 7.1 6.7 5.9 3.6 10.6 7.3 3.1 9.4 6.5

0.020 0.036 0.011 0.094 0.047 0.060 0.017 0.066 0.049 0.064 0.100 0.036

a b

Strongly perturbed alloy Weakly perturbed alloy

The unexpected properties of various dilute nitrides are incompatible with standard models (e.g. VCA) describing semiconductor alloys. Many proposals have been developed, which can be summarized in the three main models: (1) impurity band formation [137,138], (2) BAC model [139,140] and (3) a polymorphous alloy model [141,142]. The subtle distinction between the three models lies in the evolution of the localized N states and the host CB states in the alloys [143]. The impurity band model argues that the CB minimum evolves from interacting N-related impurity states (isolated N centers, N pairs and clusters) and requires no participation of higher-lying host CB states [137,138]. The BAC model includes a mutual repulsion between the N level and G-valley CB state [139,140]. N-induced perturbed host states in the third model, on the other hand, covers all host CB states that are affected by the perturbation induced by nitrogen [141,142]. There is no perfect model to fully explain the unique properties of the dilute-nitride alloys; the dispute still continues [144–146]. It has, however, been well established that the electronic energy-band consequence of such materials can be simply parameterized in terms of the BAC model [56]. If the effect of the VB is completely neglected, the N states lead to a characteristic splitting of the CB into two subbands E ðkÞ ¼

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 ðEC ðkÞ þ EN Þ ðEC ðkÞEN Þ2 þ 4V 2 x 2

ð6:20Þ

where EC(k) is the CB dispersion of the unperturbed non-nitride semiconductor, EN is the position of the N isoelectronic impurity level in that semiconductor, V is the interaction potential between the two subbands and x is the N fraction. The CB structure for GaNxAs1x obtained from Equation (6.20) with EC(0) ¼ 1.43 eV (E0), EN ¼ 1.65 eV and V ¼ 2.70 eV is shown in Figure 6.28. Any temperature dependence arises from the shift of the CB dispersion EC(0) in Equation (6.20), which is assumed to follow the Varshni, Bose–Einstein or other expression [1],

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

169

2.4

2.1

Energy (eV)

E+ 1.8

EC

EN

1.5 E0 (GaAs)

E-

GaNxAs1-x

1.2 k

Figure 6.28 CB dispersion relationships for diluted-nitride GaNxAs1x calculated from Equation (6.20). For comparison, the unperturbed GaAs CB (EC) and the position of the N level (EN) are shown

whereas EN is assumed to be independent of T. In dilute-nitride alloys the DP interaction should be treated carefully, with a view to the much weaker shift of EN with pressure. The pressure or strain dependence of the E transitions should be determined by substituting the appropriate DPs of the host semiconductor to obtain EC(k) and then deriving E(k) from Equation (6.20) or an even more detailed formalism. The effect of N incorporation on the electron effective mass is more subtle. In general, the smaller the E0 gap, the smaller the CB effective mass meG [1]. However, measurements on all diluted nitrides have shown an increase in the electron effective mass meG. The band-anticrossing-induced enhancement of the DOS electron effective mass can be calculated from the dispersion relationship E(k) in Equation (6.20) by [145] " # 2 k V x mGe ðkF Þ ¼ h2 ¼ mGe 1 þ ð6:21Þ dE ðkÞ=dkk¼kF ðEN E ðkF ÞÞ2 where meG represents the host material value at k ¼ 0. The Fermi wavevector kF and Fermi energy EF ¼ E(kF) can be determined from the free-electron concentration. Note that Equation (6.21) suggests an increase in mGe with increasing x. Since N incorporation mainly affects the CB states, the band anticrossing effect should not alter the VB structure, and as a result, the hole effective masses, appreciably. Similarly, since the band-gap bowing occurs mainly as a result of the lowering of the CB edge, a large CB offset and a small discontinuity in the VB edge should be expected. If we consider unstrained dilute nitride, the VB offset should be safely set equal to that of the host semiconductor material. The electron mobility is expected to be lower in dilute nitrides due to strong alloy or impurity scattering and the enhanced electron effective mass. It is well known that the G-valley electron mobility decreases with increasing meG [1]. Since reduced mobility of both electrons and holes has been observed, alloy or impurity scattering is likely the dominant effect governing carrier mobility, especially electron mobility.

170

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b) GaNP Nitrogen is known to form a series of isoelectronic traps in GaP. The oscillator strength of the interband transitions in N-doped GaP can be strongly enhanced by increasing N concentrations up to the alloy limit, due to N-induced admixing of the G component to the lowest CB states of the alloy leading to the crossover from an indirect gap in GaP to a direct gap in GaNxP1x with a surprisingly low N concentration of around 0.5 at% [140,147–149]. Figure 6.29(a) shows the N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxP1x. The experimental data are taken from Buyanova et al. [150]. The horizontal arrows indicate the positions of E0, EgX and EgL in the host semiconductor GaP. The solid lines represent the results calculated according to Equation (6.20) using EC(k ¼ 0) ¼ 2.76 eV (E0), EN ¼ 2.25 eV and V ¼ 3.10 eV (Table 6.19). Note that EN ¼ 2.25 eV is slightly smaller than the well-known isoelectronic NN states at 2.18 eV in GaP [151]. The determined N level EN ¼ 2.25 eV is placed nearly at the X-point CB minimum EgX ¼ 2.261 eV (Table 6.1). The EN and V values reported by Buyanova et al. [150] are, respectively, 2.25 and 2.76 eV, while those recommended by Vurgaftman and Meyer [56] are 2.18 eV (EN) and 3.05 eV (V) respectively. 3.4

2.4 (a) GaNxP1-x

3.2

2.8 E (eV)

2.2 E+

3.0

1.6 E gX

2.0 1.8

E0 E gL

2.6

1.8

2.4 E gX

2.0

X

E-

0.8

1.6 1

2 3 x (at%)

4

5

E0

0.4

0

1

2 3 x (at%)

E-

0.2

(b) GaNxAs1-x

0.6 0

E gL

0.8 0.6

1.0

4

E+

Eg

1.0

1.2 E-

1.8

1.2

E0

1.4

2.2

1.4

E+ E gL

1.6

(c) GaNxSb1-x

5

0 0

1

2 3 x (at%)

4

5

Figure 6.29 (a) N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxP1x at 300 K. The experimental data are taken from Buyanova et al. [150]. (b) N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxAs1x at 300 K. The experimental data for E are taken from Wu et al. [160] and for E þ from Gil [161]. (c) N concentration dependence of the CB edge E and G-point CB minimum E þ in GaNxSb1x at 300 K. The experimental data are taken from Jefferson et al. [178]. The solid lines in (a)–(c) represent the BAC results of Equation (6.20) using the model parameters in Table 6.19. The horizontal arrows indicate the positions of the E0, EgX and EgL gaps in the host semiconductor GaP, GaAs or GaSb

The CPs in GaNxP1x have been studied by Leibiger et al. [152] using SE at energies between 1 and 8.5 eV. They observed the G-point CPs E0 and E00 and L-direction CPs E1 and E10, together with two additional CPs labeled E21 and E22 , which cannot be assigned unambiguously. A strong blueshift of E0 and E1 was observed with increasing N incorporation, in contrast to the well-known downshift of the CB edge. The E00, E10, E21 and E22 CPs did not significantly shift with increasing N concentration.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

171

Table 6.19 BAC parameters EN and V calculated from Equation (6.20) for some dilute-nitride III–V ternaries and quaternaries at 300 K. Ternary

EN (eV)

V (eV)

Remark

GaNxP1x GaNxAs1x GaNxSb1x InNxP1x InNxAs1x InNxSb1x GaxIn1xNyAs1y

2.25 1.65 0.78 2.00 1.45 0.74 1.44 þ 0.21x

3.10 2.70 2.60 3.50 2.00 2.10 2.7 4.2x þ 3.5x2

a b c d e f g

Flit-determined from Figure 6.29 W. Shan et al., Phys. Rev. Lett. 82, 1221 (1999) c P. H. Jefferson et al., Appl. Phys. Lett. 89, 111921 (2006) d K. M. Yu et al., J. Appl. Phys. 90, 2227 (2001) e Flit-determined from Figure 6.31 f Modeled result of kp calculation shown in Figure 6.31 g I. Vurgaftman and J. R. Meyer, J. Appl. Phys. 94, 3675 (2003) a b

The CB edge E and G-point CB minimum E þ versus temperature have been measured by Ruko et al. [149] and Buyanova et al. [150]. The pressure dependence of E has also been reported [140,153]. These studies ruled out the previous assertion that the G–X transitions dominate the band gap in GaNxP1x at low N concentrations [154]. (c) GaNAs Among the dilute-nitride III–Valloys, GaNxAs1x was first grown epitaxially and represented a relatively new material system with unusual physical properties and potential technological importance [155]. A huge bowing of 18 eV was found in GaNxAs1x, which is equivalent for small N concentrations to a linear model with that slope [156]. Few attempts have been made to quantify the strong composition dependence of the band-gap energy, assuming a compositiondependent bowing parameter [157], a two-level BAC model [139,140], in the form of an arbitrary function [136,158] or a DEg/xa (a ¼ 2/3) scaling rule [159]. Figure 6.29(b) plots the fundamental gaps E and E þ as a function of x for GaNxAs1x. The experimental data for E are taken from Wu et al. [160] and for E þ from Gil [161]. The BAC results of Equation (6.20) are indicated by the solid lines. They are calculated using EN ¼ 1.65 eV and V ¼ 2.70 eV (Table 6.19) and follow the parameterization of Shan et al. [139]. The increase in E þ with increasing x is nearly equal to the band-gap reduction (DEg), indicative of a N-induced level repulsion. The CP energies versus x in GaNxAs1x were determined using SE [162–167] and PR [167,168]. These studies reported the blueshifted E1 and E1 þ D1 peaks, together with an uncommonly strong disorder-induced broadening, with increasing x. As in GaNxP1x, no clear peak shift was observed for E00 and E2 CPs [164,165,168]. A strong dependence of D0 on composition has also not been observed [169]. The linear temperature coefficient dE0/dT is 4.4 104 eV/K for GaAs at T 300 K [1]. A significant reduction in the temperature coefficient of the fundamental absorption edge has been reported for GaNxAs1x [170–173]; typically dE/dT ¼ 3 104 eV/K for x 3

172

PROPERTIES OF SEMICONDUCTOR ALLOYS

at% [170,172]. Similarly, the linear pressure coefficient dE0/dp for GaAs is 1.2 101 eV/ GPa [1], while a value for dE/dp of 7 102 eV/GPa was observed for GaNxAs1x with x ¼ 0.1 at% at T ¼ 33 130 K [174]. Such weak external perturbation dependence of E in GaNxAs1x is in good agreement with the BAC model [145]. The GaNxAs1x alloy at high N concentration is an attractive material for extending the wavelength range of GaN-based optoelectronic devices toward the red/IR region. The fundamental absorption edges of such As-poor (N-rich) alloys have been studied by several authors [156,175,176]. These results are shown in Figure 6.30 together with those obtained in the As-rich region [160]. The solid line shows the quadratic fit given by (E in eV) E ¼ 1:4311:7x þ 13:5x2

ð6:22Þ

3.5 3.0

c-GaNxAs1-x

2.5 2.0 E- (eV)

1.5

Quadratic fit BAC model

1.0 0.5 0 -0.5 -1.0 -1.5

semimetallic 0

0.2

0.4

x

0.6

0.8

1.0

Figure 6.30 Lowest absorption edge E versus x for c-GaNxAs1x at 300 K. The experimental data are taken from Wu et al. [160] (open circles), Kimura et al. [175] (solid triangles) and Wu et al. [176] (open triangles). The solid line represents the quadratic least-squares fit of Equation (6.22), while the dashed line shows the BAC result of Equation (6.19) using the model parameters in Table 6.19

This fit provides huge bowing of c ¼ 13.5 eV and thus results in a semimetallic overlap of the CB and VB at the intermediate compositions 0.15 x 0.73. It should be noted, however, that the 0.4 eV band-gap reduction observed with x 3 at% in Figure 6.30 is similar to that measured with an N fraction of x 15 at% [177]. No upper limit for the N concentrations for which the BAC model remains valid, has been identified so far [56]. (d) GaNSb There has been only one experimental report on the structural and optoelectronic properties of GaNxSb1x by MBE [178]. The GaNxSb1x layers (0.002 x 0.01) were grown on GaAs substrates. The band-gap energies were determined from FTIR measurements. The band-gap reduction DEg was solely due to the substitution of dilute amounts of highly electronegative N for Sb, and was greater than that observed in GaNxAs1x with the same N concentration. The results obtained by Jefferson et al. are shown in Figure 6.29(c) [178]. The solid lines show the fits of these data with Equation (6.20). The parameters determined using the BAC model are listed in Table 6.19.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

173

(e) InNP Several experiments have been carried out on InNxP1x [179,180]. Bi and Tu [179] incorporated N atoms into InP by gas-source MBE using N radicals and observed the linear reduction DEg with increasing N concentration. The value of DEg is about 0.15 eV at x ¼ 1 at%. More recently, Yu et al. [180] obtained dilute-nitride InNxP1x films by N þ ion implantation into InP with N doses up to 4.8 at%. The InNxP1x layers were thermally stable up to an annealing temperature of 850 C. The data of Yu et al. are shown in Figure 6.31(a) [180]. These data are nearly the same as those obtained by Bi and Tu [179]. The solid lines represent the BAC model results calculated using Equation (6.20) and the numeric parameters in Table 6.19. (f) InNAs There have been several experimental studies on the band-gap reduction in InNxAs1x [181– 184]. All these studies showed that the band gap was reduced with increasing x, as shown in Figure 6.31(b). The solid lines in Figure 6.31(b) represent the results calculated using

2.6 2.4

E gX

E+

2.2 E gL

E (eV)

2.0 1.8 1.6 1.4

E0

1.2 E-

1.0 0.8 0.6 0

(a) InNxP1-x 1

2 3 x (at%)

4

2.0 1.4 1.8 (b) InNxAs1-x 1.2 1.6 1.0 E+ X 1.4 0.8 Eg 1.2 0.6 E gL 1.0 0.4 0.8 0.2 0.6 0 E0 0.4 -0.2 0.2 -0.4 E0 -0.6 semimetallic -0.2 -0.8 5 0 1 2 3 4 5 0 x (at%)

E gL

E+

(c) InNxSb1-x E0

Esemimetallic

2

4 6 x (at%)

8

10

Figure 6.31 (a) N concentration dependence of the CB edge E and G-point CB minimum E þ in InNxP1x at 300 K [180]. (b) N concentration dependence of the CB edge E and G-point CB minimum E þ in InNxAs1x at 300 K [181–184]. (c) N concentration dependence of the CB edge E and G-point CB minimum E þ in InNxSb1x at 300 K. The solid lines in (a) and (b) and dashed lines in (c) represent the BAC results of Equation (6.20) using the model parameters in Table 6.19, while the solid lines in (c) show kp calculation made by Veal et al. [187]. The horizontal arrows indicate the positions of the E0, EgX and EgL gaps in the host semiconductor InP, InAs or InSb

Equation (6.20) with EN ¼ 1.45 eV and V ¼ 2.00 eV (Table 6.19). The effective N level EN ¼ 1.45 eV is nearly equal to those reported by Shih et al. [182] and Veal et al. [184] (1.48 eV). The interaction potential V ¼ 2.00 eV is slightly larger than those in Shih et al. [182] (1.68 eV), Kuroda et al. [183] (1.86 eV) and Veal et al. [184] (1.77 eV). The higher-lying CPs E1 and E1 þ D1 in InNxAs1x were studied using SE [185]. They were blue-shifted at a rate of 20–25 meV/at%[N].

174

PROPERTIES OF SEMICONDUCTOR ALLOYS

(g) InNSb Murdin et al. [186] measured the electron effective mass near the band anticrossing point by CR in InNxSb1x with the absorption edge near 15 mm. The observed results directly demonstrate band anticrossing and quantitatively confirm an increase in the effective mass predicted by a tight binding calculation for low N concentration (x < 1 at%). More recently, Veal et al. [187] formed a thin InNxSb1x layer by low-energy N implantation on InSb and found from XPS that N occupies 6 at% of the anion sublattice sites. Using HREELS, they also observed the absence of a depletion layer, indicating that the Fermi level is located below the VB maximum. Consequently, the CB minimum is located below the VB maximum, meaning that a negative band-gap material has been formed. These results are consistent with the kp calculation that predicts a semimetallic band structure, as shown by the solid lines in Figure 6.31(c) [187]. The dashed lines in Figure 6.31(c) show the parameterization fits of the kp results (solid lines) using Equation (6.20). The resulting parameters are found to be EN ¼ 0.74 eV and V ¼ 2.10 eV (Table 6.19).

Table 6.20 Energies for some indirect and direct gaps in some Al–(V, V) tenaries at 300 K Ternary

Band gap

Expression (eV)

Remark

AlPxAs1x

EgX EgL E0 EgX EgL E0 EgX EgL E0

2.15 0.07x þ 0.40x2 2.37 þ 0.82x þ 0.38x2 3.01 þ 0.77x þ 0.13x2 1.615 þ 0.588x þ 0.277x2 2.211 þ 0.603x þ 0.756x2 2.27 0.49x þ 2.13x2 1.615 þ 0.285x þ 0.250x2 2.211 0.315x þ 0.474x2 2.27 0.45x þ 1.19x2

a a b a a b a a b

AlPxSb1x

AlAsxSb1x

Bowing parameter is obtained from a theoretical study by A.-B. Chen and A. Sher (Semiconductor Alloys. Plenum, New York, 1995) b Bowing parameter is estimated from Equation (6.23) a

6.3.6 Al–(V, V) Alloy The minimum gaps in the Al-based III–V ternaries AlPxAs1x, AlPxSb1x and AlAsxSb1x are an indirect band gaps throughout their whole composition range with the CB minimum located in the vicinity of the X point, as shown in Figure 6.32. The various curves have been calculated from the data in Table 6.20. The bowing parameters c for E0 are estimated from the product of the lattice constant and electronegativity differences (Equation (6.23)). The bowing parameters c for EgL and EgX are obtained from the theoretical calculations by Chen and Sher [188]. Very few studies have been carried out on the determination of the energy-band structures for the Al–(V, V) ternaries. Saadallah et al. [189] have studied the photothermal properties of an MBE-grown AlAs0.08Sb0.92/GaSb layer. From the absorption spectrum they obtained, we can

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

175

4

(c) AlAsx Sb1-x

E0,E gID (eV)

3

2

E0 EgX EgL

1

(a) AlPx As1-x 0 AlP

(b) AlAsx Sb1-x AlAs

AlSb

AlP

x

Figure 6.32 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlPxAs1x, (b) AlAsxSb1x and (c) AlPxSb1x at 300 K. The solid circle in (b) is estimated from an optical absorption spectrum by Saadallah et al. [189]. The various curves in (a)–(c) represent the calculated results using the data in Table 6.20

estimate an absorption edge at 800 nm (1.55 eV). The solid circle in Figure 6.32(b) represents this data.

6.3.7 Ga–(V, V) Alloy (a) GaPAs GaPxAs1x remains a direct gap material in the composition range 0 x 0.48 at room temperature. Above x 0.48, the alloy becomes indirect because the X-valley minimum crosses below the G-valley minimum. The bowing parameter for E0 reported previously lies within a relatively narrow range c ¼ 0.174–0.21 eV [89]. The lowest direct and indirect gaps for GaPxAs1x as determined by ER [190] and PL measurements [191], respectively, are shown in Figure 6.33(a). The c ¼ 0.24 eV value for EgX recommended by Vurgaftman et al. [89] lies approximately in the middle of the previously reported range of 0.20–0.28 eV. The same authors also recommended a value of c ¼ 0.16 eV for EgL. The higher-lying CPs, such as E1, E1 þ D1, E00, E00 þ D00, E2 and E2 þ d, in GaPxAs1x have been determined by ER [190], reflectivity [192] and SE [193]. The kinks in the slope of the composition dependence of E1 and E1 þ D1 are found at x 0.5 [190,192]. A recent SE study does not confirm such an anomaly, but observes some alloy disorder effects, i.e. a large positive bowing for E0 and a large reduction in the E1/(E1 þ D1) strengths at x 0.5 [193]. The large bowing reported is c ¼ 0.54 eV, which is larger by more than a factor of 2 than the commonly accepted values (0.20–0.28 eV). This large bowing effect has not been verified and relies on only two data points with intermediates at x ¼ 0.4 and 0.7. All CPs higher than E1/(E1 þ D1) showed an almost linear increase with x [190,192,193], as shown in Figure 6.33(b). The recommended band-gap expressions are listed in Table 6.21. The temperature effects on the fundamental absorption edge especially near the E0 EgX crossover region in GaPxAs1x were studied using PL [191,194] and optical absorption [195]. As the temperature was increased to above 77 K, marked changes in PL were observed for both

176

PROPERTIES OF SEMICONDUCTOR ALLOYS 3.0

6

E2

(a) 5

E0 '

4

EgL EgX

2.0

E gD (eV)

E0,E gID (eV)

2.5

E0

E1+∆1 E1

3 2

E0+∆0

E0

1.5

GaPx As1-x 1.0 0

0.2 0.4 0.6 0.8 1.0 x

1 0 0

(b) 0.2 0.4 0.6 0.8 1.0 x

Figure 6.33 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaPxAs1x at 300 K. The experimental data are taken for E0 from Thompson et al. [190] (open circles) and for EgX from Craford et al. [191] (solid circles). (b) Energies of some CPs versus x for GaPxAs1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.21

N-doped and N-free alloys [191]. In both cases the higher-energy or near-band-edge process dominated the emission as the temperature was increased. Zero-phonon as well as phononassisted transitions were identified in the intrinsic absorption edge [195]. (b) GaPSb There are very few reports relating to GaPxSb1x in the literature [196,197]. The intrinsic absorption edge in GaPxSb1x as a function of x obtained by PL measurements is shown in

Table 6.21 Energies for some direct and indirect gaps in GaPxAs1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

1.43 þ 1.14x þ 0.19x2 1.72 þ 0.75x þ 0.16x2 1.76 þ 0.90x þ 0.18x2 1.910 þ 0.111x þ 0.240x2 2.89 þ 0.82x 3.13 þ 0.69x 4.52 þ 0.22x 5.13 þ 0.15x2

a a b a c c c c

Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) Bowing parameter is fit-determined from experimental data reported by A. G. Thomson et al. (Phys. Rev. 146, 601 (1966)) c Bowing parameter (c ¼ 0 eV) is obtained from A. G. Thompson et al. (Phys. Rev. 146, 601 (1966)) and K. J. Kim et al. (J. Appl. Phys. 84, 3696 (1998)) a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

177

Figure 6.34(a) [196,197]. The solid lines represent the E0, EgX and EgL versus x data obtained by putting c ¼ 2.7 eV into Equation (A.5). This bowing parameter is taken from Vurgaftman et al. [89]. Although the experimental data scatter largely, the curves of the calculated results explain the experimental data very well. From Figure 6.34(a), we can expect the E0 EgX crossover to occur at x 0.4. 3.0 2.5

6

(b)

GaPx Sb1-x

5

E2

E0 EgL

1.5

E0 '

4 E gD (eV)

E0, E gID (eV)

2.0

EgX

E1+∆1

3

E1

1.0

2

0.5

1

E0+∆0 E0

(a) 0 0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.34 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaPxSb1x at 300 K. The experimental data are taken from Jou et al. [196] and Loualiche et al. [197] (solid circles). (b) Energies of some CPs versus x for GaPxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.22

There have been no reports published concerning the higher-lying CPs in GaPxSb1x. We, therefore, assume the bowing parameters for E1 and E1 þ D1 to be a half of that for E0 and those for E00 and E2 to be a quarter of that for E0. Such trends can be found in some III–V ternary alloys (see e.g. GaAsxSb1x in Table 6.23). The solid lines in Figure 6.34(b) show the calculated results using the data in Table 6.22. Table 6.22 Energies for some direct and indirect gaps in GaPxSb1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL EgX E0 þ D0 E1 E1 þ D1 E00 E2

0.72 0.66x þ 2.70x2 0.76 0.83x þ 2.70x2 1.050 1.489x þ 2.700x2 1.50 1.36x þ 2.70x2 2.05 þ 0.31x þ 1.35x2 2.50 0.03x þ 1.35x2 3.56 þ 0.50x þ 0.68x2 4.14 þ 0.46x þ 0.68x2

a a a b c c d d

Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) Postulated bowing parameter equal to that for E0 c Bowing parameter is assumed to be a half of that for E0 (c ¼ 1.35 eV) d Bowing parameter is assumed to be a quarter of that for E0 (c ¼ 0.68 eV) a b

178

PROPERTIES OF SEMICONDUCTOR ALLOYS

(c) GaAsSb GaAsxSb1x remains a direct gap material over the whole composition range, as shown in Figure 6.35(a). The E0-gap bowing parameter has been determined using various techniques [89]. The experimental data plotted in Figure 6.35(a) were obtained from PL results by Nahory et al. [198] (solid circles) and from optical absorption measurements by Yano et al. [199] (open circles) and McGlinn et al. [200] (solid triangles). The quadratic fit of these data provides c ¼ 1.25 eV for E0. This value is slightly smaller than that recommended by Vurgaftman et al. [89] (c ¼ 1.43 eV). No experimental data are available for the c values of EgX and EgL . In Figure 6.35(a), the x-dependent EgX and EgL curves are calculated by introducing c ¼ 1.20 eV into Equation (A.5). These bowing parameters are recommended by Vurgaftman et al. [89]. 2.0

6

(a)

(b) 5

E2 EgX

1.0

EgL

E0 '

4 E gD (eV)

E0, E gID (eV)

1.5

E0

3

E1+∆1 E1

2

E0+∆0

0.5 1

GaAsx Sb1-x 0

0

0.2

0.4

E0 0.6

x

0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.35 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for GaAsxSb1x at 300 K. The experimental data are taken from Nahory et al. [198] (solid circles), Yano et al. [199] (open circles) and McGlinn et al. [200] (solid triangles). (b) Energies of some CPs versus x for GaAsxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.23

The higher-lying CPs have been investigated on MBE-grown GaAsxSb1x (0.56 x 1.0) on GaAs(100) substrates using PR [201] and those (0.35 x 0.78) grown on InP(100) substrates by MOCVD using SE [202]. Serries et al. [203] determined strained and relaxed E1/ (E1 þ D1) energies before and after correction for strain effects. The sample thickness used by Ferrini et al. [201] was in the range 0.6–1 mm for complete strain release at each mole fraction. The results obtained by these authors [201,203], together with those for E0 and E0 þ D0 (Table 6.23) are shown in Figure 6.35(b). The temperature dependence of E0 in GaAsxSb1x has been studied by several authors [203– 205]. Lukic-Zrnic et al. [204] obtained the Varshni parameters a and b, which describe not only their own data well, but also the previous data of Merkel et al. [203]. More recently, Chouaib et al. [205] obtained the Varshni parameters a¼(4.0 0.1) 104 ((3.9 0.1) 104) eV/K and b ¼ 143 18 (140 14) K for unintentionally doped (Si-doped) GaAsxSb1x/InP. These values are in reasonable agreement with those obtained by Lukic-Zrnic et al. [204]. Note that GaAsxSb1x can be grown lattice-matched to InP at x 0.5.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

179

Table 6.23 Energies for some direct and indirect gaps in GaAsxSb1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL EgX E0 þ D0 E1 E1 þ D1 E00 E2

0.72 0.54x þ 1.25x2 0.76 0.24x þ 1.20x2 1.05 0.34x þ 1.20x2 1.50 0.99x þ 1.25x2 2.05 þ 0.29x þ 0.55x2 2.50 þ 0.04x þ 0.59x2 3.56 þ 0.64x þ 0.32x2 4.14 þ 0.80x þ 0.19x2

a b b c d d e e

Flit-determined from Figure 6.35 Bowing parameter is obtained from I. Vurgaftman et al. (J. Appl. Phys. 89, 5815 (2001)) c Postulated bowing parameter equal to that for E0 d Bowing parameter is obtained from D. Serries et al. (J. Appl. Phys. 87, 8522 (2000)) e Bowing parameter is obtained from R. Ferrini et al. (J. Appl. Phys. 86, 4706 (1999)) a b

6.3.8 In–(V, V) Alloy (a) InPAs Due to the high vapor pressure of As and P elements, growth of InPxAs1x from the melt has received very little attention. Antypas and Yep [206] prepared InPxAs1x (0.735 x 1.0) by LPE and undertook PL measurements. Nicholas et al. [207] also grew InPxAs1x layers (0 x 1.0) by CVD and obtained their optical absorption spectra. More recently, Wada et al. [208] carried out both PL and absorption measurements on InPxAs1x layers (0.33 x 1.0) grown by MOCVD on InP(100) substrates. The E0 values for InPxAs1x obtained by these authors have been plotted in Figure 6.36(a). From these data, the bowing parameter c ¼ 0.145 eV for E0 can be obtained. Note, however, that the most recent data produced by Bui et al. [209] using PR, showed clear upward bowing of c ¼ 0.22 eV. Figure 6.36(a) also shows the composition dependence of EgX and EgL calculated from Equation (A.5) with the same c value as that for E0 (0.145 eV). ER measurements were carried out on InPxAs1x by Vishnubhatla et al. [129] and Thompson et al. [210]. Choi et al. [211] also used SE to investigate the band structure of InPxAs1x films on InP(100). The composition dependence of the higher-lying CPs, such as E1, E1 þ D1, E00 and E2 CPs, was determined from such investigations. Figure 6.36(b) shows the results of Vishnubhatla et al. [129]. Table 6.24 summarizes the numeric expressions. The temperature variation of E0 in InPxAs1x has been studied by Wada et al. [208]. The linear temperature coefficient dE0/dT for InP and InAs was reported to be 3.3 104 and 4.2 104 eV/K, respectively [1]. The InPxAs1x value obtained by Wada et al. is approximately 3 104 eV/K and is independent of x. (b) InPSb InPxSb1x may be an alternative material to Al-based semiconductor alloys, which commonly suffer from carbon and oxygen impurities. However, the predicted miscibility gap of this alloy

180

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.5

6

InPx As1-x

5

2.0

E0 '

4

1.5 E gD (eV)

E0,E gID (eV)

E gX

E2

E gL 1.0

E0 0.5

3

E1+∆1 E1

2 1

E0+∆0 E0

(a) 0 0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

x

0.4

0.6

(b) 0.8

1.0

x

Figure 6.36 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for InPxAs1x at 300 K. The experimental data are taken from Antypas and Yep [206] (solid circles), Nicholas et al. [207] (open circles) and Wada et al. [208] (solid triangles). (b) Energies of some CPs versus x for InPxAs1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.24

could limit its usefulness in device applications. Reihlen et al. [212] succeeded in growing InPxSb1x epilayers on InP, InAs and InSb by MOCVD and examined their optical properties. Duncan et al. [213] also grew an InPxSb1x/InP epilayer and obtained E0 ¼ 0.6 eVat 300 K from PL measurements. These results are shown in Figure 6.37(a). The least-squares fit of these data gives a bowing parameter of c ¼ 1.60 eV. This value is slightly smaller than c ¼ 1.9 0.1 eV obtained at 10 K by Jou et al. [196]. The solid lines in Figure 6.37(a) show the composition dependence of EgX and EgL and have been obtained by putting the same c values for E0 (1.60 eV) into Equation (A.5) since to date no alternative reliable data have been published.

Table 6.24 Energies for some direct and indirect gaps in InPxAs1x at 300 K Band gap

Expression (eV)

Remark

E0 E0 þ D0 EgL EgX E1 E1 þ D1 E00 E2

0.359 þ 0.846x þ 0.145x2 0.726 þ 0.589x þ 0.145x2 1.070 þ 0.835x þ 0.145x2 1.370 þ 0.695x þ 0.145x2 2.50 þ 0.42x þ 0.25x2 2.78 þ 0.26x þ 0.25x2 4.44 þ 0.24x þ 0.02x2 4.70 þ 0.37x þ 0.03x2

a b b b c c c c

Flit-determined from Figure 6.36 Postulated bowing parameter equal to that for E0 c Bowing parameter is obtained from S. S. Vishnubhatla et al. (Can. J. Phys. 47, 1661 (1969))

a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS 6

3.0

5 4

2.0 E gD (eV)

E0,E gID (eV)

(b)

InPx Sb1-x

2.5

EgX

1.5

E gL

1.0

3

E2 E0 ' E1+∆1 E1

2

E0

0.5

1

E0+∆0

(a) 0

181

0

0.2

0.4

0.6

0.8

E0 1.0

0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.37 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for InPxSb1x at 300 K. The experimental data are taken from Reihlen et al. [212] (solid circles) and Duncan et al. [213] (open circle). (b) Energies of some CPs versus x for InPxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.25

Since there have been no published reports relating to the higher-lying CPs in InPxSb1x, let us, therefore, assume the bowing parameters for E1 and E1 þ D1 to be a half of that for E0 and those for E00 and E2 to be a quarter of that for E0 (see Section 6.3.7(b)). The solid lines in Figure 6.37(b) represent the calculated results using such bowing parameters. The recommended band-gap expressions are summarized in Table 6.25. (c) InAsSb InSb has the smallest band gap among the III–V binary semiconductors (E0 ¼ 0.17 eV at 300 K). The InAsxSb1x alloy has the lowest band gap among all III–V semiconductors, with values as small as 0.1 eV at room temperature. The bowing parameter c for E0 previously Table 6.25 Energies for some direct and indirect gaps in InPxSb1x at 300 K Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.17 0.42x þ 1.60x2 0.93 0.48x þ 1.60x2 1.04 1.18x þ 1.60x2 1.63 1.02x þ 1.60x2 1.80 þ 0.57x þ 0.80x2 2.30 þ 0.19x þ 0.80x2 3.26 þ 1.04x þ 0.40x2 3.90 þ 0.80x þ 0.40x2

a b b b c c d d

Flit-determined from Figure 6.37 Postulated bowing parameter equal to that for E0 c Bowing parameter is assumed to be a half of that for E0 (c ¼ 0.80 eV) d Bowing parameter is assumed to be a quarter of that for E0 (c ¼ 0.40 eV) a b

182

PROPERTIES OF SEMICONDUCTOR ALLOYS

reported for InAsxSb1x is 0.6 eV [89]. The values of E0 as a function of x for InAsxSb1x have been plotted in Figure 6.38(a). The experimental data have been obtained from Woolley and Warner [214], Stringfellow and Greene [215] and Dobbelaere et al. [216]. The least-squares fit of these data gives c ¼ 0.600 eV. The composition dependence of EgX and EgL obtained from Equation (A.5) using the same bowing parameter as that for E0 (c ¼ 0.60 eV) have also been plotted in Figure 6.38(a). 2.0

6 InAsx Sb1-x

(a)

(b) 5

EgX

EgL

1.0

E2

4 E gD (eV)

E0, E gID (eV)

1.5

3 2

0.5

E0 ' E1+∆1 E1

1

E0

E0+∆0 E0

0 0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

x

0.4

0.6

0.8

1.0

x

Figure 6.38 (a) Energies of the lowest direct E0 and indirect gaps EgID versus x for InAsxSb1x at 300 K. The experimental data are taken from Woolley and Warner [214] (open circles), Stringfellow and Greene [215] (open triangles) and Dobbelaere et al. [216] (solid circles). (b) Energies of some CPs versus x for InAsxSb1x at 300 K. The solid lines in (a) and (b) represent the calculated results using the data in Table 6.26

SE was used to investigate the higher-lying CPs in InAsxSb1x [217]. The x-dependent E1, E1 þ D1 and E2 CPs were determined from this study. These results, together with those for E0 and E0 þ D0 CPs, are shown in Figure 6.38(b) and summarized in Table 6.26. Table 6.26 Energies for some direct and indirect gaps in InAsxSb1x at 300 K. LI ¼ linear interpolation. Band gap

Expression (eV)

Remark

E0 EgL E0 þ D0 EgX E1 E1 þ D1 E00 E2

0.170 0.411x þ 0.600x2 0.93 0.46x þ 0.60x2 1.04 0.914x þ 0.600x2 1.63 0.86x þ 0.60x2 1.8 þ 0.7x 2.30 þ 0.48x 3.26 þ 1.18x 3.9 þ 0.8x

a b b b c c LI e

Flit-determined from Figure 6.38 Postulated bowing parameter equal to that for E0 c Bowing parameter (c ¼ 0 eV) is obtained from H. Y. Deng and N. Dai (Phys. Rev. B 73, 113102 (2006))

a b

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

183

The Varshni parameters for E0 in InAs (InSb) are reported to be a ¼ 3.07 104 eV/K (2.7 104 eV/K) and b ¼ 191 K (106 K) [1]. The Varshni parameters for InAsxSb1x have also been determined by a number of authors, although the alloy composition was limited to a narrow region (see e.g. [218–222]). These data give the Varshni parameters of a 2.4 104 eV/K and b 180 K both of which are nearly independent of x, although the alloy composition was in the limited range x 0.06 or x 0.799. Only the data of Bansal et al. [220] gave the extremely large values of a ¼ 7.1 104 eV/K and b ¼ 675 K for x ¼ 0.05.

6.3.9 Summary This section has concentrated on reviewing the lowest direct and indirect gaps, together with some higher-lying CPs in III–V ternary alloys. These energy gaps have an approximately quadratic dependence on the mole fraction of one endpoint material x. The main emphasis is thus on the nonlinear or bowing parameter c. The lowest direct (E0) and indirect gaps (EgX ) versus composition x for some cubic III–V ternary alloys are shown in Figure 6.39. The degree of bowing varies quite considerably depending on the band gap in question. The large, positive bowing effect obtained in the VCA is largely a volume effect [4]. An impressive plot of a large parabola composed of the individual E0 versus x plots is shown in Figure 6.39 (AlAs–GaAs– –GaSb–AlSb). 5

E0, E gID (eV)

4

UV (He-Cd)

3

Blue (He-Cd) Green (Ar) Red (He-Ne)

2 E gX

IR (Nd3+:YAG)

1 E0

0 AlAs

GaAs

InAs

InSb

GaSb

AlSb

AlAs

AlP

GaP

InP

InN

GaN

AlN

x

Figure 6.39 Lowest direct E0 and indirect gaps EgX versus composition x for some cubic IIIV semiconductor ternary alloys at 300 K. The experimental data are shown by the open circles

Table 6.27 summarizes the bowing parameters c for E0, EgX and EgL in some (III, III)–V and III–(V, V) ternary alloys. The degree of bowing does not appear to be directly related to the binary energy steps. Figure 6.40 shows these parameters plotted against the product DaabDXab of the lattice constant and electronegativity differences between the endpoint binaries a and b. The electronegativity differences were obtained from Phillips’ data [46]. The solid line in Figure 6.40 represents the least-squares fit given by (c in eV, DaabDXab in AeV) c ¼ 9:62ðDaab DXab Þ

ð6:23Þ

Note that the proportionality factor 9.62 A1 in Equation (6.23) is slightly smaller than that 1 (9.93 A ) obtained in Equation (6.8). The c values for the Al–(V, V) ternary alloys shown in Table 6.20 are calculated from Equation (6.23).

184

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 6.27 Bowing parameters c for E0, EgX and EgL in some (III, III)–V and III–(V, V) ternaries (in eV) Ternary

E0

EgX

EgL

Ternary

E0

EgX

EgL

(Al, Ga)P (Al, In)P (Ga, In)P (Al, Ga)As (Al, In)As (Ga, In)As (Al, Ga)Sb (Al, In)Sb (Ga, In)Sb

0 0.40 0.65 0.127b 0.72 0.58 0.044b 0.43 0.415

0 0 0.200 0.055 0 0.70 0 0 0.33

0 0 0.34 0 0 0.50 0 0 0.40

Al(P, As) Al(P, Sb) Al(As, Sb) Ga(P, As) Ga(P, Sb) Ga(As, Sb) In(P, As) In(P, Sb) In(As, Sb)

0.13a 2.13a 1.19a 0.19 2.70 1.25 0.145 1.60 0.60

0.40 0.277 0.250 0.240 2.700 1.20 0.145 1.60 0.60

0.38 0.756 0.474 0.16 2.70 1.20 0.145 1.60 0.60

a b

Estimated from Equation (6.23) In the limit x ! 0 (see e.g. Equation (6.12))

3.0 2.5

GPS

c (eV)

2.0 IPS

1.5 GAS 1.0 GIP GIA

0.5 GPA 0

AlIA IAS AlIP

GIS AlIS

IPA 0

0.05

0.10

0.15

0.20

0.25

∆aAB∆XAB (ÅeV)

Figure 6.40 Bowing parameter c of the G-valley gap E0 versus product DaabDXab of the lattice-constant and electronegativity differences between the endpoint binary materials a and b in some IIIV semiconductor ternary alloys. The solid line represents the calculated result using Equation (6.23). G ¼ Ga; I ¼ In; A ¼ As; S ¼ Sb

6.4 III–V SEMICONDUCTOR QUATERNARY ALLOY 6.4.1 Dilute-nitride Quaternary Alloy (a) AlGaNAs The energy gaps in dilute-nitride AlxGa1xNyAs1y have been investigated by Shan et al. [180]. The energy positions of E and E þ can be explained by assuming an anticrossing interaction between states at the G minimum and located N state EN whose energy depends on x in the

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

185

following manner EN(x) ¼ 1.65 þ 0.61x eV. The E þ transitions lie above the G-valley CB minimum even in the indirect gap region of the AlxGa1xAs matrix. The results indicate that the N-induced interactions between the extended G, L and X CB states do not play a significant role in the modification of the CB structure of dilute-nitride III–V alloys. (b) GaInNP Some studies on GaxIn1xNyP1y have been carried out using PL [223,224] and PR [225,226]. All these studies suggested that N incorporation reduces the fundamental absorption edge of GaxIn1xP. The BAC parameters are EN ¼ 2.1 0.1 eV and V ¼ 1.7 0.2 eV for x ¼ 0.44–0.49 [224] and EN ¼ 2.040 eVand V ¼ 1.449 0.170 eV for x ¼ 0.46 [226]. A somewhat weaker temperature dependence of the band-gap energy was reported by Buyanova et al. [224], but Lin and Hwang [226] were unable to confirm such a weak temperature dependence. (c) GaInNAs Vurgaftman and Meyer [56] reviewed the results of studies on GaxIn1xNyAs1y. The addition of N narrows the band gap for lower In concentrations, while at the same time providing tensile strain compensation. Samples with very low In compositions in the order of 10 at% showed no significant difference from GaNxAs1x apart from the expected GaxIn1xAs gap decrease including bowing [56,89]. However, for samples with larger In contents grown on GaAs and InP, an alternative parameterization with the BAC model was proposed [227]. The interaction potentials V recommended for GaNxAs1x and InNxAs1x are 2.70 and 2.00 eV, respectively (Table 6.19). Pan et al. [228] took EN to be independent of the In concentration and used V ¼ 2.5 eV for GaxIn1xNyAs1y with x ¼ 0.7–0.9. Choulis et al. [229] made the same assumption regarding EN, but the interaction potential was considerably lower (V ¼ 1.675 eV). A similar value (V ¼ 1.7 eV) was independently proposed by Polimeni et al. [230] for x ¼ 0.24–0.41. On the other hand, Sun et al. [231] used V ¼ 2.8 3.0 eV to explain PL and PLE spectra in GaxIn1xNyAs1y/GaAs QWs (x ¼ 27.2 at%). Serries et al. [232] also obtained the V values for high In-containing GaxIn1xNyAs1y/InP films and showed the QWs to be only slightly smaller than that reported for low In-content GaxIn1xNyAs1y/GaAs films. Vurgaftman and Meyer [56] suggested x-dependent EN and V values for GaxIn1xNyAs1y and these values are summarized in Table 6.19. The higher-lying CPs in GaxIn1xNyAs1y have been studied using SE [233]. In strong contrast to the behavior of E and E þ , the higher-lying CPs such as E1 and E2 showed very weak liner nonlinearity with the N concentration. The temperature dependence of the fundamental absorption edge in GaxIn1xNyAs1y has also been studied by several authors [234–237] and found to exhibit weaker dependence than that observed in the N-free GaxIn1xAs matrix [234,235]. The pressure dependence of the fundamental absorption edge in GaxIn1xNyAs1y has been studied experimentally by several authors [139,234,238]. These results show a very much weaker pressure dependence than those observed in the N-free GaxIn1xAs alloy. (d) GaNPAs GaNxPyAs1xy were synthesized by N ion implantation into a GaPyAs1y epilayer (y ¼ 0 0.35) followed by pulsed-laser melting and rapid thermal annealing techniques [239]. As

186

PROPERTIES OF SEMICONDUCTOR ALLOYS

predicted from the BAC model, the incorporation of N split the CB in the bulk GaPyAs1y substrate, and relatively strong optical transitions from the VB to the lower (E) and upper (E þ ) conduction subbands were observed.

6.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs AlxGa1xPyAs1y lattice-matches to GaAs with x and y are given in Table 1.10. The AlxGa1xPyAs1y layers can also be grown on commercially available GaP0.39As0.61 epitaxial substrates. The lattice-matching relationship between x and y for the AlxGa1xPyAs1y/ GaP0.39As0.61 system can be written as y¼

0:079 þ 0:008x 0:2030:005x

ð0 x 1:0; 0:39 y 0:44Þ

ð6:24Þ

No detailed experimental data relating to the x-dependent band-gap energies in AlxGa1xPyAs1y have been published thus far. The E0, EgX and EgL values obtained from Equation (A.15) are plotted in Figure 6.41 as a function of x for (a) AlxGa1xPyAs1y/GaAs and (b) AlxGa1xPyAs1y/GaP0.39As0.61. The ternary bowing parameters are taken from Table 6.27, while the quaternary parameter DAlGaPAs is assumed to be zero. We can see that the E0 EgX crossing occurs at x 0.36 (Figure 6.41(a)) and at 0.07 (Figure 6.41(b)) (see also Table 6.28). 3. 5

3. 0

3.5 (a)

(b) 3.0 E0

E0, E gID (eV)

2. 0

1. 5

E0, E gID (eV)

E gL

2. 5

E gX E0

1. 0

2.5

E gL

2.0

E gX

1.5

1.0

0. 5

0.5 Alx Ga1-x Py As1-y /GaAs

0 0

0.2

0.4

0.6 x

Alx Ga1-x Py As1-y /GaPAs 0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.41 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlxGa1xPyAs1y/ GaAs and (b) AlxGa1xPyAs1y/GaP0.39As0.61 calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaPAs ¼ 0 eV

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

187

Table 6.28 Energy for the fundamental absorption edge (Eg) in III–V quaternaries at 300 K. The expression gives the quadratic fit of Equation (A.15) with DABCD ¼ 0 eV Quaternary

Substrate

Eg

Expression (eV)

AlxGa1xPyAs1y

GaAs

E0 EgX E0 EgX E0 EgX E0 EgX E0 EgX E0 EgX E0 EgL EgX E0 EgX E0 E0 E0 E0 E0 E0 EgX E0 E0

1.43 þ 1.50x þ 0.11x2 1.91 þ 1.93x þ 0.04x2 1.90 þ 1.42x þ 0.06x2 1.99 þ 0.18x þ 0.03x2 0.72 þ 1.46x þ 0.06x2 1.05 þ 0.54x þ 0.05x2 0.77 þ 1.53x þ 0.09x2 1.19 þ 0.65x þ 0.01x2 0.68 þ 1.48x þ 0.07x2 1.03 þ 0.60x þ 0.04x2 0.30 þ 1.17x þ 0.77x2 1.33 þ 0.68x 0.36x2 0.88 þ 0.88x þ 0.63x2 1.45 þ 0.30x þ 0.44x2 1.53 þ 0.53x 0.21x2 0.359 þ 1.143x þ 0.722x2 1.37 þ 0.57x 0.26x2 1.43 þ 0.30y þ 0.18y2 0.75 þ 0.46y þ 0.14y2 0.28 0.16x þ 0.60x2 0.97 0.84x þ 0.64x2 0.359 0.415x þ 0.718x2 1.90 þ 0.57x þ 0.10x2 2.25 þ 0.09x 0.01x2 0.75 þ 0.68x þ 0.06x2 0.512 þ 0.030y 0.183y2

GaPAs AlxGa1xAsySb1y

GaSb InP InAs

AlxIn1xAsySb1y

GaSb InP

InAs GaxIn1xPyAs1y

(AlxGa1x)0.53In0.47P

GaAs InP GaSb InP InAs GaAs

(AlxGa1x)0.48In0.52As InPxAsySb1xy

InP InAs

GaxIn1xAsySb1y

Remark

0.48 x 1.0 0.48 x 1.0 0.48 x 1.0

a b c 0.47 x 1.0 d d e f

Quadratic-fit result of Equation (A.15) with DAlInAsSb ¼ 0.11 eV Fit-determined from Figure 6.44 c Fit-determined from Figure 6.47 d Fit-determined from Figure 6.49 e dit-determined from Figure 6.50 f Fit-determined from Figure 6.51 a b

(b) AlGaAsSb AlxGa1xAsySb1y can be grown lattice-matched to GaSb, InP and InAs. The corresponding x and y relationships are presented in Table 1.10. This material system is attractive for optoelectronic applications in the near-IR wavelength range. However, very little data have so far been available on the composition-dependent band-gap energies in this alloy system. Herrera-Perez et al. [240] grew LPE-AlxGa1xAsySb1y layers (x ¼ 0.27, y ¼ 0.02) on GaSb (100) and determined from PR measurements the energy gaps to be 1.05 eV. Yacobi et al. [241] also obtained an absorption edge of 0.975 eV for (x, y) ¼ (0.15, 0.13) using a photothermal method. More recently, Saadallah et al. [189] undertook a photothermal study on an MBE-AlxGa1xAsySb1y/GaSb layer (x ¼ 0.70, y ¼ 0.08) and obtained an absorption edge

188

PROPERTIES OF SEMICONDUCTOR ALLOYS

of 1.57 eV. These data are plotted in Figure 6.42(a). The solid and dashed lines show the results calculated using Equation (A.15) together with the ternary bowing parameters shown in Table 6.27 and assuming DAlGaAsSb ¼ 0 eV. The quadratic fits of these curves are summarized in Table 6.28. Filho et al. [242] measured the temperature-dependent PL peak energies for an MBEAlxGa1xAsySb1y/InP layer (x ¼ 0.12, y ¼ 0.51) at T ¼ 10 180 K. By extrapolating these data, we can estimate the PL peak to be 0.89 eVat 300 K. This data is shown in Figure 6.42(b), together with the calculated data from Equation (A.15) (see also Table 6.28). The calculated E0, EgX and EgL values versus x curves for AlxGa1xAsySb1y/InAs in Figure 6.42(c) are very similar to those in Figure 6.42(a). This is not surprising in view of the near equality of the InAs and GaSb lattice parameters. Yacobi et al. [241] found the As composition for AlxGa1xAsySb1y at x ¼ 0.15 grown on GaSb substrate to be y ¼ 0.13. However, the exact lattice-matching relationship suggests that Yacobi’s sample (x, y) ¼ (0.15, 0.13) has y composition closely lattice-matched to InAs (y ¼ 0.10) rather than to GaSb (y ¼ 0.01). This data is, therefore, not only shown in Figure 6.42(a) but also in Figure 6.42(c). 2.5

2.5

(a)

2.5

(b)

2.0

(c)

2.0

2.0

E0,E gID (eV)

E gL

1.5

E gL

E gL E gX

1.0

E gX

1.5 1.0

E0

1.5 1.0

E0

0.5

E0

0.5 Alx Ga1-x Asy Sb1-y /GaSb

0 0

E gX

0 0.2 0.4 0.6 0.8 1.0 0 x

0.5 Alx Ga1-x Asy Sb1-y /InP

0 0.2 0.4 0.6 0.8 1.0 0 x

Alx Ga1-x Asy Sb1-y /InAs

0.2 0.4 0.6 0.8 1.0 x

Figure 6.42 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlxGa1xAsySb1y/ GaSb, (b) AlxGa1xAsySb1y/InP and (c) AlxGa1xAsySb1y/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaAsSb ¼ 0 eV

No clear bowing can be seen for E0 in Figure 6.42. The Al0.5Ga0.5AsxSb1x layers (x ¼ 0.3 0.7) grown on GaAs by MBE have also been studied by PL [243]. A discrepancy of up to 0.2 eV from the predicted value using the established formalism indicates that an extra bowing factor needs to be included in the E0 versus x expression for this quaternary system. The temperature dependence of the fundamental absorption edges has been studied for AlxGa1xAsySb1y/GaSb (x ¼ 0.27, y ¼ 0.02) [240] and AlxGa1xAsySb1y/InP (x ¼ 0.12, y ¼ 0.51) [242]. The Varshni parameters for AlxGa1xAsySb1y/GaSb were a ¼ 3.6 104 eV/K and b ¼ 78 K [240], which are considerably smaller than the endpoint binary values a ¼ (3.6 5.5) 104 eV/K and b ¼ 204 234 K [1]. (c) AlInAsSb AlxIn1xAsySb1y can be grown lattice-matched to GaSb, InP and InAs (Table 1.10). However, no detailed study has been carried out on AlxIn1xAsySb1y lattice-matched to GaSb and InP.

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

189

There is only one study by Charykov et al. [244] which reports PL measurements on LPEAlxIn1xAsySb1y/InAs epilayers. The composition range investigated corresponds to a wavelength from 3 (x ¼ 0) to 2.5 mm (x ¼ 0.08). The solid and dashed lines in Figure 6.43 show the calculated E0, EgX and EgL gaps as a function of x for AlxIn1xAsySb1y lattice-matched to GaSb, InP and InAs. These are obtained from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlInAsSb ¼ 0 eV. The quadratic fits of these curves are summarized in Table 6.28. The solid circles in Figure 6.43(c) represent the experimental data taken from Charykov et al. [244]. The direct–indirect crossover occurs at xc ¼ 0.77 in (a), 0.70 in (b) and 0.77 in (c). 2.5

2.5

(a)

2.5

(c)

(b)

2.0

2.0

2.0

E0, E gID (eV)

E gX

1.5

E gX

1.5

E gL

1.5

E gX

E0

1.0

E gL

E0

0.5

1.0 0.5

AlxIn1-xAsySb1-y /GaSb

0 0

1.0

0.2 0.4 0.6 0.8 1.0 x

E0

0.5 AlxIn1-xAsySb1-y /InP

0 0

E gL

0.2 0.4 0.6 0.8 1.0 x

AlxIn1-xAsySb1-y /InAs

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.43 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) AlxIn1xAsySb1y/ GaSb, (b) AlxIn1xAsySb1y/InP and (c) AlxIn1xAsySb1y/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlInAsSb ¼ 0 eV. The experimental data in (c) are taken from Charykov et al. [244]

(d) GaInPAs A number of experimental studies have been published on E0 versus composition for GaxIn1xPyAs1y quaternary alloy. These studies concentrated on the technologically important compositions which have lattice parameters equal to that of InP [245]. GaxIn1xPyAs1y can also be grown lattice-matched to GaAs. However, not very much is known about GaxIn1xPyAs1y/GaAs. Shirakata et al. [246] performed ER measurements on LPE-grown GaxIn1xPyAs1y/GaAs with y ¼ 0.70 and 0.96. These data are plotted versus y in Figure 6.44(a). The experimental data for GaxIn1xPyAs1y/InP are gathered from various sources and plotted in Figure 6.44(b). The solid and dashed lines in Figure 6.44 are obtained from Equation (A.15) using the ternary bowing parameters in Table 6.27 and inputting DAlInAsSb ¼ 0.11 (E0) and 0 eV (EgX and EgL ). The quaternary parameter DAlInAsSb ¼ 0.11 eV is taken from Donati et al. [247]. This parameter explains the E0 data plotted in Figure 6.44(a), but not that in Figure 6.44(b). The heavy solid line in Figure 6.44(b) shows the quadratic least-squares fit of E0. The bowing parameter of c ¼ 0.14 eV is determined from this fit (Table 6.28). The higher-lying CPs, such as E0 þ D0, E1, E1 þ D1, E00 and E2, for GaxIn1xPyAs1y/InP have been investigated by many authors [245,248,249]. The recommended higher-lying CPs are listed in Table 6.29 (see also Figure 6.45(a)).

190

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.5

2.5 (a)

2.0

EgX E0,E gID (eV)

E0,E gID (eV)

2.0

Gax In1-x Py As1-y /InP

EgL

E0

1.5

1.0

EgL

EgX 1.5 E0 1.0

Gax In1-x Py As1-y /GaAs 0.5

0

(b)

0.2 0.4 0.6 0.8 1.0 y

0.5 0

0.2 0.4 0.6 0.8 1.0 y

Figure 6.44 Energies of the lowest direct E0 and indirect gaps EgID versus y for (a) GaxIn1xPyAs1y/ GaAs and (b) GaxIn1xPyAs1y/InP calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DGaInPAs ¼ 0.11 (E0) and 0 eV ðEgX Þ and ðEgL Þ. The heavy solid line in (b) shows the quadratic least-squares fit listed in Table 6.28

6

6

6

(a) E 0′

5

E gD (eV)

4

E1+∆1 E1

2

E0+∆0 1

E1

3

E0+∆0

2

E0

0

5

E2

4

E 0′

3 2 1

1 Gax In1-x Py As1-y /InP

0

E2

5 4

3

(AlxGa1-x)0.48In0.52As/InP

(b)

(AlxGa1-x)0.53In0.47P/GaAs

0

0.2 0.4 0.6 0.8 1.0 0 y

0

0.2 0.4 0.6 0.8 1.0 0 x

E1+∆1 E1

E0+∆0 E0

(c)

0.2 0.4 0.6 0.8 1.0 x

Figure 6.45 Energies of the higher-lying CPs versus y or x for (a) GaxIn1xPyAs1y/InP, (b) (AlxGa1x)0.53In0.47P/GaAs and (c) (AlxGa1x)0.48In0.52As/InP. The functional forms are summarized in Tables 6.28 and 6.29

The temperature dependence of E0 for GaxIn1xPyAs1y/InP has been studied by several authors [245]. The experimental dE0/dT versus y data are shown in Figure 6.46(a). These data give the slowly varying function of dE0/dT versus y (in 104 eV/K)

dE0 ¼ 3:6 þ 0:5y dT

ð6:25Þ

The pressure coefficient dE0/dp for GaxIn1xPyAs1y/InP has been studied by several authors [245]. These results are summarized in Figure 6.46(b). The corresponding y dependence is written as (in 102 eV/GPa)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

191

Table 6.29 Energies for the higher-lying CPs in some III–V quaternaries at 300 K Quaternary

Substrate

CP

GaxIn1xPyAs1y

InP

E0 þ E1 E1 þ E00 E0 þ E1 E2 E0 þ E1 E1 þ E00 E2

(AlxGa1x)0.53In0.47P

GaAs

(AlxGa1x)0.48In0.52As

InP

Expression (eV) D0

1.08 2.56 2.85 4.42 1.98 3.23 4.80 1.10 2.55 2.83 4.36 4.74

D1 D0 D0 D1

dE0 ¼ 11:33:0y dp

þ þ þ þ þ þ þ þ þ þ þ þ

0.30y þ 0.08y2 0.34y þ 0.27y2 0.25y þ 0.19y2 0.27y þ 0.01y2 0.62x þ 0.10x2 0.37x þ 0.09x2 0.02x 0.64x þ 0.18x2 0.36x þ 0.11x2 0.39x þ 0.08x2 0.69x 0.48x2 0.15x 0.13x2

ð6:26Þ

(e) GaInAsSb Figure 6.47 shows E0, EgX and EgL versus x for GaxIn1xAsySb1y lattice-matched to GaSb, InP and InAs. A distinguishing feature of GaxIn1xAsySb1y is the existence of a wide immiscibility range 0.24 < x < 0.75, which means that the alloy can be prepared only in a narrow range of compositions either adjoining GaSb (x ¼ 1.0) or InAs (x ¼ 0). The solid and dashed lines in Figure 6.47 are calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DGaInAsSb ¼ 0 eV.

6

15

(a) dE120 /dp (10-2 eV/GPa)

-dE0 /dT (10-4 eV/K)

5 4 3 2

6 3

1 0

9

GaxIn1-xPyAs1-y/InP 0

0.2 0.4 0.6 0.8 1.0 y

(b) 0 0

0.2 0.4 0.6 0.8 1.0 y

Figure 6.46 (a) Temperature and (b) pressure coefficients of E0 as a function of y for GaxIn1xPyAs1y/ InP. The solid lines in (a) and (b) are obtained from Equations (6.25) and (6.26), respectively

192

PROPERTIES OF SEMICONDUCTOR ALLOYS 2.0

2.0 Gax In1-x Asy Sb1-y /GaSb

E0, E gID (eV)

1.5

2.0 Gax In1-x Asy Sb1-y /InP

1.5

1.5

E gX E gL

EgX

1.0

1.0

EgL E0

0.5

E0

0.5

(a)

0 0

EgX

1.0

EgL

0.5

Gax In1-x AsySb1-y /InAs

0 0.2 0.4 0.6 0.8 1.0 0 x

E0

(b)

(c)

0 0.2 0.4 0.6 0.8 1.0 0 x

0.2 0.4 0.6 0.8 1.0 x

Figure 6.47 Energies of the lowest direct E0 and indirect gaps EgID versus x for (a) GaxIn1xAsySb1y/ GaSb, (b) GaxIn1xAsySb1y/InP and (c) GaxIn1xAsySb1y/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DGaInAsSb ¼ 0 eV. The heavy solid line in Figure 6.47(a) shows the quadratic least-squares fit listed in Table 6.28

The open circles in Figure 6.47 show the experimental data taken from various sources [250– 254]. It can bee seen that Equation (A.15) shows reasonable agreement with the available experimental data. However, Figure 6.47(a) shows poor agreement. We, therefore, tried to least-squares fit these data using a quadratic function. The heavy solid line in Figure 6.47(a) shows this result. The determined bowing parameter is c ¼ 0.60 eV (Table 6.28). The temperature dependence of the G-valley gap E0 has been studied by Iyer et al. [255] and Mu~ noz et al. [256] for GaxIn1xAsySb1y grown on GaSb and by Gong et al. [257] for GaxIn1xAsySb1y grown on InAs. These results are shown in Figure 6.48. Although the data are somewhat sparse, they give values of dE0/dT 3.8 104 and 4.0 104 eV/K for samples grown on GaSb and InAs, respectively, near 300 K. 8 7

GaxIn1-xAsySb1-y

-dE0 /dT (10-4 eV/K)

6 5 on InAs 4 3

on GaSb

2 1 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.48 Temperature coefficient dE0/dT as a function of x for GaxIn1xAsySb1y lattice-matched to GaSb and InAs

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

193

6.4.3 (III, III, III)–V Alloy (a) AlGaInP AlxGayIn1xyP has the largest direct band gap of any semiconductor lattice-matched to GaAs. There have been many reports on (AlxGa1x)0.53In0.47P/GaAs (see e.g. [258–260]). The open circles in Figure 6.49 represent the experimental data at 300 K. They are taken from various sources, e.g. Asami et al. [261], Cao et al. [262] and Adachi et al. [263]. Data for E0, EgX and EgL for (AlxGa1x)0.53In0.47P/GaAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaInP ¼ 0 eV have been plotted in Figure 6.49.

3.0

E gL

E0, E gID (eV)

2.5

E gX E0

2.0

(AlxGa1-x)0.53In0.47P/GaAs 1.5 0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.49 Energies of the lowest direct E0 and indirect gaps EgID versus x for (AlxGa1x)0.53In0.47P/ GaAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaInP ¼ 0 eV. The heavy solid lines show the quadratic least-squares fit listed in Table 6.28

Equation (A.15) predicts that the G–X crossover occurs at xc ¼ 0.55. However, excellent agreement can be never achieved with the experimental data even if DAlGaInP 6¼ 0 eV is introduced into Equation (A.15). We, therefore, fit the experimental E0 and EgX data using a quadratic function with respect to x. The heavy solid lines in Figure 6.49 show these results (see also Table 6.28) and predict that the G–X crossover point will be at xc ¼ 0.64. No experimental data has, however, been reported on the G–X crossover point. The higher-lying CPs as a function of x for (AlxGa1x)0.53In0.47P/GaAs have been determined using various techniques, such as ER [261,263], TR [264] and SE [260,264,265]. The E0 þ D0, E1 and E2 energies versus x for (AlxGa1x)0.53In0.47P/GaAs have been plotted in Figure 6.45(b). They are obtained by averaging the published experimental data and are summarized in Table 6.29.

194

PROPERTIES OF SEMICONDUCTOR ALLOYS

The pressure dependence of E0 for (AlxGa1x)0.53In0.47P/GaAs has been investigated by several authors [266,267]. The experimental data reported by Harada et al. [267] can be written as dE0 dE0 ð0Þ ¼ ð10:29xÞ dp dp

ð6:27Þ

where dE0(0)/dp ¼ 9.5 eV/GPa is the Ga0.5In0.5P (x ¼ 0) value estimated from the linear interpolation between GaP and InP [1]. (b) AlGaInAs AlxGayIn1xyAs can be relatively easily grown on InP by MBE. This alloy system can also be prepared by MOCVD [268]. The E0, EgX and EgL gaps for (AlxGa1x)0.48In0.52As/InP are shown in Figure 6.50. The alloy system remains a direct gap material over the whole composition range 0 x 1.0. The open circles in Figure 6.50 represent the experimental E0 data taken from various sources (see e.g. [268–271]). These data are found to be slightly smaller than those calculated from Equation (A.15) assuming DAlGaInAs ¼ 0 eV. The heavy solid line in Figure 6.50 represents the quadratic least-squares fit (Table 6.28).

2.0

E gX

E0, E gID (eV)

1.5 EgL 1.0

E0

0.5 (AlxGa1-x)0.48In0.52As/InP 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.50 Energies of the lowest direct E0 and indirect gaps EgID versus x for (AlxGa1x)0.48In0.52As/ InP calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DAlGaInAs ¼ 0 eV. The heavy solid line shows the quadratic least-squares fit listed in Table 6.28

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

195

The higher-lying CPs in (AlxGa1x)0.48In0.52As/InP have been studied using ER [272] and SE [273]. The E0 þ D0, E1, E1 þ D1, E00 and E2 versus x data for (AlxGa1x)0.48In0.52As/InP as determined by ER [272] has been plotted in Figure 6.45(c). The corresponding expressions are summarized in Table 6.29.

6.4.4 III–(V, V, V) Alloy InPxAsySb1xy/InAs is the only quaternary system that has been well studied in the literature. The E0 versus y data for InPxAsySb1xy/InAs are shown in Figure 6.51. They are taken from various sources [213,274–276]. The solid and dashed lines also show the E0, EgX and EgL versus y curves obtained from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DInPAsSb ¼ 0 eV. The heavy solid line is obtained from the quadratic least-squares fit. This fit gives considerable upward bowing of c ¼ 0.183 eV for E0 (Table 6.28).

2.0

E gX

E0,E gID (eV)

1.5 E gL 1.0

E0 0.5 InPxAsySb1-x-y /InAs 0

0

0.2

0.4

y

0.6

0.8

1.0

Figure 6.51 Energies of the lowest direct E0 and indirect gaps EgID versus y for InPxAsySb1xy/InAs calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and assuming DInPAsSb ¼ 0 eV. The heavy solid line shows the quadratic least-squares fit listed in Table 6.28

The higher-lying CPs, E0 þ D0, E1 and E1 þ D1, in InPxAsySb1xy/InAs have been determined using ER [274,275]. Like E0, these CPs show no strong dependence on alloy composition. The temperature dependence of E0 has also been determined to be (2.2–2.9) 104 eV/K for 0.46 y 1.0 [275], suggesting little dependence on alloy composition.

196

PROPERTIES OF SEMICONDUCTOR ALLOYS

6.4.5 Summary The lowest direct (E0) and indirect gaps (EgX ) for some III–V quaternary alloys lattice-matched to (a) GaAs, (b) GaSb, (c) InP and (d) InAs are summarized in Figure 6.52. The limits of applicability of the linear interpolation scheme using the binary data are apparent. The rationalized biquadratic interpolation algorithm, Equation (A.15), can be safely used to estimate the band-gap energies in quaternary alloys. However, it tends to give energies that are smaller (Figures 6.44, 6.47 and 6.50) or larger than the experimental data (Figures 6.49 and 6.51). These poorer fits can be improved to some extent, if the nonzero DABCD parameter is inserted into Equation (A.15). For example, introducing DGaInPAs ¼ 0.5 eV into Equation (A.15) improves the fit considerably, as demonstrated in Figure 6.53. It is, however, very difficult to explain the origin of such large upward bowing in this alloy system (GaxIn1xPyAs1y/InP). The alloying effect in certain types of (III, III)–(V, V) quaternaries may be a secondary effect of the relatively strong cation–cation and anion–anion sublattice disorders which occur in ternary alloys. The triple cation or anion disorder effect may also be much smaller in alloys of the type (III, III, III)–Vor III–(V, V, V). We can, therefore, expect that Equation (A.15) will become a good tool for obtaining reliable quaternary parameters when more exact ternary bowing parameters, which can be introduced into Equation (A.15), are required.

2.5

(b) GaSb

(c) InP

(d) InAs

E0,E gX (eV)

2.0 1.5 1.0 0.5

(a) GaAs 0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x (y) x x (y) x (y) GaxIn1-xPyAs1-y (y) (AlxGa1-x)0.53In0.47P

AlxGa1-xAsySb1-y AlxIn1-xAsySb1-y GaxIn1-xAsySb1-y

AlxGa1-xAsySb1-y AlxIn1-xAsySb1-y GaxIn1-xPyAs1-y (y) GaxIn1-xAsySb1-y (AlxGa1-x)0.48In0.52As

AlxGa1-xAsySb1-y AlxIn1-xAsySb1-y GaxIn1-xAsySb1-y InPxAsySb1-x-y (y)

Figure 6.52 Energy of the lowest band gap E0 or EgX versus x (or y) for some IIIV quaternary alloys lattice-matched to (a) GaAs, (b) GaSb, (c) InP and (d) InAs. These curves are calculated from the data in Table 6.28

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

197

1.4

1.2

E0 (eV)

DGaInPAs =+1.5eV 1.0

0.8

-0.5 eV Gax In1-x Py As1-y /InP

0.6 0

0.2

0.4

y

0.6

0.8

1.0

Figure 6.53 Lowest band-gap energy E0 versus y for GaxIn1xPyAs1y/InP at 300 K. The solid lines are calculated from Equation (A.15) using the ternary bowing parameters in Table 6.27 and varying DGaInPAs from 0.5 to þ 1.5 eV in steps of 0.5 eV

6.5 II–VI SEMICONDUCTOR ALLOY 6.5.1 (II, II)–O Ternary Alloy (a) BeZnO Beryllium chalcogenides attracted considerable attention because they exhibit covalent bonding, and appear to have very large band gaps. However, their optical and electronic properties have not yet been fully clarified. Both BeO and ZnO usually crystallize in the wurtzite structure. BeO has a wide band gap (E0 ¼ 10.6 eV). Studies on BexZn1xO are very limited. Ryu et al. [277] deposited BexZn1xO layers on sapphire substrates using a hydride beam deposition method. They measured the transmittance spectra at 300 K and obtained E0 for 0 x 0.69. More recently, Han et al. [278] used the same crystal growth and measurement techniques, and obtained E0 up to x ¼ 0.28. These data are shown in Figure 6.54(a) (open circles [277], solid circles [278]). The solid line shows a rough fit of these data using the quadratic function shown in Table 6.30. (b) MgZnO MgO is the prototype of an ionic semiconductor crystallizing in the rocksalt structure, whereas ZnO crystallizes in the wurtzite structure. There have been many studies on the electronic energyband structure of MgxZn1xO. The E0 versus x data taken from various sources (see e.g. [279– 283]) are shown in Figure 6.54(b). It can be seen that the E0 data for x 0.5 are a good fit with the linear function of x, while those for x > 0.4 show quadratic dependence on x. The corresponding expressions are listed in Table 6.30. The wurtzite–cubic mixed phase region occurs at around x 0.4.

198

PROPERTIES OF SEMICONDUCTOR ALLOYS 12

8

(b) MgxZn1-xO

(c) ZnxCd1-xO

7

10 wurtzite

9 E0 (eV)

4.0

(a) BexZn1-xO

11

3.5 rocksalt

6

8

3.0

7

rocksalt

5 wurtzite

6

2.5

4

5 4

mixed phase

3

3 2

2 0

0.2 0.4 0.6 0.8 1.0 x

2.0 wurtzite

1.5 0

0.2 0.4 0.6 0.8 1.0 x

0

0.2 0.4 0.6 0.8 1.0 x

Figure 6.54 Energy of the E0 gap versus x for some (II, II)–O ternaries at 300 K: (a) BexZn1xO, (b) MgxZn1xO and (c) ZnxCd1xO. The solid lines represent the calculated results using the data in Table 6.30

The composition dependence of the higher-lying CPs in w-MgxZn1xO has been studied using SE [280]. E1 and E2 energies were observed at 7 and 9 eV, respectively, and showed little dependence on x. The pressure dependence of E0 has been measured using a diamond anvil cell for p up to 10 GPa [284]. The experimental pressure coefficient dE0/dp increased at a rate of 40x meV/GPa (0 x 0.13). (c) ZnCdO There have been a few reports on ZnxCd1xO [285,286]. The E0 versus x data measured by Ishihara et al. [285] (solid circles) and Wang et al. [286] (open circles) have been plotted in Figure 6.54(c) These plots show that E0 in the wurtzite region varies quadratically with x (0.2 x 1.0, see Table 6.30). The E0 value in the rocksalt region decreases with decreasing x. The E0 versus x data at 2.1 K have been determined using PL [287]. The temperature dependence of E0 has also been established by Makino [279] for T ¼ 5–300 K (x ¼ 0.01) and Wang et al. [286] for T ¼ 6–300 K (x ¼ 0.022, 0.09 and 0.157), illustrating nearly the same behavior as that for ZnO [279].

6.5.2 (II, II)–S Ternary Alloy (a) MgZnS Under normal conditions MgS crystallizes in the rocksalt structure, whereas ZnS crystallizes either in the wurtzite or zinc-blende structure. ZnS has the largest band gap among II–VI semiconductors except for Be- and Mg-chalcogenides. The E0 gap in w-MgxZn1xS has been investigated by means of optical absorption [288]. The samples used were grown on (0001)sapphire substrates by PLD. These data are shown in Figure 6.55(a) by the solid circles. It can

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

199

Table 6.30 Energy for E0 in some II–VI ternaries and quaternaries at 300 K. w ¼ wurtzite; rs ¼ rocksalt; zb ¼ zinc-blende Alloy BexZn1xO MgxZn1xO ZnxCd1xO MgxZn1xS ZnxCd1xS ZnxHg1xS CdxHg1xS BexZn1xSe BexCd1xSe MgxZn1xSe MgxCd1xSe ZnxCd1xSe CdxHg1xSe BexZn1xTe MgxZn1xTe MgxCd1xTe ZnxCd1xTe ZnxHg1xTe CdxHg1xTe ZnOxS1x ZnSxSe1x ZnSxTe1x ZnSexTe1x CdSxSe1x CdSxTe1x CdSexTe1x MgxZn1xSySe1y/GaAs MgxZn1xSeyTe1y/InP BexMgyZn1xySe/GaAs MgxZnyCd1xySe/InP

E0 (eV) 3.4 2.1x þ 9.3x2 3.4 þ 2.3x 7.2 5.0x þ 5.6x2 1.76 0.11x þ 1.75x2 3.81 þ 0.65x 3.75 þ 0.80x 2.460 þ 0.439x þ 0.827x2 2.501 þ 0.328x þ 0.921x2 0.040 þ 2.770x þ 0.996x2 0.040 þ 2.541x 2.721 þ 1.846x þ 1.033x2 1.675 þ 0.925x þ 3.000x2 2.721 þ 0.679x þ 0.600x2 1.675 þ 2.125x þ 0.200x2 1.751 þ 2.349x 1.675 þ 0.659x þ 0.387x2 0.08 þ 1.57x 2.27 þ 1.83x 2.27 þ 0.67x þ 0.46x2 1.51 þ 1.35x þ 0.54x2 1.51 þ 0.45x þ 0.31x2 0.15 þ 1.96x þ 0.46x2 0.15 þ 1.45x þ 0.21x2 3.75 4.85x þ 4.50x2 2.721 þ 0.425x þ 0.580x2 2.270 2.294x þ 3.750x2 2.270 1.049x þ 1.500x2 1.751 þ 0.050x þ 0.700x2 1.51 0.85x þ 1.80x2 1.560 0.859x þ 1.800x2 1.510 0.673x þ 0.838x2 2.749 þ 1.340x þ 0.650x2 2.13 þ 1.59x þ 0.37x2 2.79 þ 1.44y þ 1.74y2 2.11 þ 1.57x þ 0.40x2

Remark w (0 x 1.0) w (0 x 0.5) rs (0.4 x 1.0) w (0.2 x 1.0) zb (0 x 0.25), T ¼ 10 K w (0 x 0.25) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) w (0.6 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 0.32) w (0 x 1.0) zb (0 x 1.0) zb (0 x 0.8) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) w (0 x 1.0) zb (0 x 1.0) zb (0 x 0.5) zb (0 x 0.84) zb (0 y 0.67) zb (0 x 0.83)

be seen that E0 increases almost linearly at a rate of 0.8x eV from E0 ¼ 3.75 eV at x ¼ 0 (wZnS). The detailed expression is given in Table 6.30. The zinc-blende MgxZn1xS layers for x up to 0.24 have been grown on GaP(100) by MBE [289]. The E0 gaps for these layers are determined by low-temperature (10 K) PL measurements. These results are shown in Figure 6.55(a) by the open circles. As in the case of w-MgxZn1xS, the E0 gap in c-MgxZn1xS increases at a rate of 0.7x eV from E0 ¼ 3.81 eVat x ¼ 0 (c-ZnS). From the extrapolation scheme E0 4.5 eV for c-MgS is estimated to occur at 10 K.

200

PROPERTIES OF SEMICONDUCTOR ALLOYS 4.1

3.8 3.6

E0 (eV)

zinc-blende 4.0 (T=10 K)

3.4 3.2

4

(b) ZnxCd1-xS

3

(c) ZnxHg1-xS 3

wurtzite cubic

(d) CdxHg1-xS 2 zincblende

2

3.9

1 3.0 wurtzite

wurtzite

1

2.8

3.8

0

(a) MgxZn1-xS

2.6

0 zinc-blende

mixed phase

3.7 2.4 -1 -1 0 0.1 0.2 0.3 0.4 0.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x x

Figure 6.55 Energy of the E0 gap versus x for some (II, II)–S ternaries at 300 K: (a) MgxZn1xS, (b) ZnxCd1xS, (c) ZnxHg1xS and (d) CdxHg1xS. The solid and dashed lines represent the calculated results using the data in Table 6.30

(b) ZnCdS ZnxCd1xS can be grown both in the wurtzite and zinc-blende structures. The E0 versus x data for w-ZnxCd1xS reported in the literature [2–293] are shown in Figure 6.55(b). The experimental data largely scatter. The solid line shows the least-squares fit of these data (see Table 6.30). This fit gives a bowing parameter of c 0.921 eV. Yokogawa et al. [294] estimated c 0.827 eV for E0 in c-ZnxCd1xS. Introducing this value into Equation (A.5), the composition dependence of E0 for c-ZnxCd1xS can be calculated. The dashed line in Figure 6.55(b) represents the result of this calculation (see also Table 6.30). The temperature coefficient of E0 for w-ZnxCd1xS has been studied by means of electroabsorption spectroscopy [295]. The experimental dE0/dT is in the range of (3.8–6.0) 104 eV/K for x ¼ 0–1.0. The pressure coefficient dE0/dp in w-ZnxCd1xS has also been determined for p up to 15 GPa [291]. The linear pressure coefficient, when plotted against the Cd concentration, displays a slow decrease up to 25 at% at which concentration a sudden drop appears. This behavior is reminiscent of ‘percolation-type’ phenomena. (c) ZnHgS The complete solid solution was obtained throughout the whole range for the ZnS–HgS alloy system [296]. The reflectance measurements revealed that the zinc-blende ZnxHg1xS alloy appears to show a nearly linear increase of E0 from x 0.44 to 1.0. These results are shown in Figure 6.55(c) [296]. The solid line shows the quadratic fit of these data and those for x ¼ 0 and 1.0 (see also Table 6.30). (d) CdHgS CdS and HgS form solid solutions over the whole range, but the crystal structure depends on the composition. The zinc-blende solid solution c-CdxHg1xS is obtained in the x ¼ 0–0.4 range, while the wurtzite solid solution w-CdxHg1xS is obtained for x 0.6. The cubic and wurtzite

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

201

structures can be present in the x ¼ 0.4–0.6 range. As expected, the ratio of cubic to wurtzite solid solution increases continuously with increasing HgS concentration [296,297]. The dependence of E0 on x for CdxHg1xS is shown in Figure 6.55(d) [296]. We can see that the E0 versus x data are satisfactorily interpreted by the linear interpolation scheme between the CdS (2.541 eV) and HgS values (0.04 eV), as shown by the solid line.

6.5.3 (II, II)–Se Ternary Alloy (a) BeZnSe Figure 6.56(a) shows the E0 versus x data for BexZn1xSe obtained using SE by Wilmers et al. [298] (solid circles) and Bukaluk et al. [299] (open circles). The solid line represents the quadratic least-squares fit of these data. The bowing parameter c is determined to be 1.033 eV (Table 6.30). 6

6

(a) BexZn1-xSe 5

E0, E gX (eV)

5

4 4 3

4.5

(b) BexCd1-xSe

EgX

(c) MgxZn1-xSe 4.0

zinc-blende

EgX

3.5 3

E0

2 zinc-blende

3.0 E0

EgX E0

zinc-blende

2 1 2.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x 3.0 2 4 (d) MgxCd1-xSe (e) ZnxCd1-xSe (f) CdxHg1-xSe

E0 (eV)

wurtzite

2.5

3

2

5 4 3 2 zb 1 0 0.5 1.0

2.0

zinc-blende

1

0

zinc-blende

wurtzite mixed phase

1 1.5 -1 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x

Figure 6.56 Energy of the E0 gap versus x for some (II, II)–Se ternaries at 300 K: (a) BexZn1xSe, (b) BexCd1xSe, (c) MgxZn1xSe, (d) MgxCd1xSe, (e) ZnxCd1xSe and (f) CdxHg1xSe. The solid lines represent the calculated results using the data in Table 6.30. The dashed lines in (a)–(c) show the x dependence of EgX obtained by the linear interpolation between the endpoint binary data in Table 6.1. The dotted line in (d) represents the liner least-squares fit, which predicts a value of E0 3.8 eV for w-MgSe (x ¼ 1.0). The inset in (d) shows the x dependence of E0 in c-MgxCd1xSe (see also Table 6.30)

Beryllium chalcogenides BeX (X ¼ S, Se, Te) are characterized by an indirect band gap with the CB minimum lying at the X point [300]. The direct and indirect gaps of these materials are listed in Table 6.1. The dashed line in Figure 6.56(a) shows the x dependence of EgX for

202

PROPERTIES OF SEMICONDUCTOR ALLOYS

BexZn1xSe obtained by the linear interpolation between ZnSe (x ¼ 0) and BeSe (x ¼ 1.0). We can expect the G–X crossover to occur at x 0.4. This agrees with an abrupt drop in the main PL peak intensity at x 0.45 [301,302]. The SE spectra for BexZn1xSe have been measured in the 2–30 eV range [298], the 1.25–5 eV range [299] and the 1.5–6.0 eV range [303]. The higher-lying CPs assigned to E0 þ D0, E1, E1 þ D1, E2, E00 and E10 can be seen [298] and with increasing Be content their spectral positions are systematically shifted toward higher energies. Each CP has a different slope dEg/dx, E0 and E0 þ D0 having the steepest slope and, as a result, having the largest bowing parameter. The highest CP peak is at 8.5 eV (E10 ) [298]. (b) BeCdSe The zinc-blende-type BexCd1xSe alloy can be epitaxially grown on III–V semiconductor substrates. E0 values for c-BexCd1xSe epilayers grown on GaAs(100) [304] and on InP(100) have been reported [305,306]. The experimental data obtained from these studies are shown in Figure 6.56(b). The solid line shows a quadratic dependence of E0 on x (Table 6.30). The dashed line also shows the predicted EgX values obtained by the linear interpolation between c-CdSe (x ¼ 0) and BeSe (x ¼ 1.0). The G–X crossover is expected to occur at x 0.8. The E0 value in w-BexCd1xSe has also been measured by Huang et al. [306] and Wronkowska et al. [307]. (c) MgZnSe Bulk MgxZn1xSe crystals grown by the Bridgman method are known to show the sphalerite–wurtzite phase transition at x ¼ 0.185 0.03 [308]. On the other hand, c-MgxZn1xSe epilayer can be grown over the whole alloy range (0 x 1.0). The E0 versus x data for cMgxZn1xSe reported in the literature [309–312] are shown in Figure 6.56(c). The quadratic least-squares fit produces a bowing of c 0.600 eV for E0 (Table 6.30). The dashed line represents the x dependence of EgX obtained by the linear interpolation between ZnSe (x ¼ 0) and MgSe (x ¼ 1.0). It can be seen that the G–X crossover occurs at x 0.55. No experimental determination has, however, been reported until now. The higher-lying CPs in c-MgxZn1xSe have been studied using SE for x 0.37 [303] and x 0.21 [311]. The E0 þ D0, E1 and E1 þ D1 CPs are reported to increase almost linearly with increasing x. The temperature dependence of E0 has been studied for both c-MgxZn1xSe [313,314] and w-MgxZn1xSe [315]. The experimental data have been analyzed using semi-empirical formulas, such as the Varshni and P€assler formulas [1]. An anomalous temperature dependence, i.e. showing a positive temperature coefficient at T 70 K, has also been found in bulk w-MgxZn1xSe crystals grown by a closed-tube sublimation method and analyzed as originating from a volume dilution effect due to deep-level defects [315]. (d) MgCdSe Under normal conditions bulk MgxCd1xSe crystallizes in the wurtzite structure. The E0 versus x data for w-MgxCd1xSe obtained from Wronkowska et al. [316] (open circles), Firszt et al. [317] (open triangles) and Kim et al. [318] (solid circles) are shown in Figure 6.56(d); the experimental data scatter largely. The dotted line represents the linear least-squares fit of these data, which gives a change of E0 at a rate of dE0/dx ¼ 2.071 eV and predicts a value of E0 3.8 eV for w-MgSe. This value is considerably smaller than that of c-MgSe (E0 ¼ 4.0 eV,

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

203

Table 6.1). In III–Vand II–VI semiconductors, the wurtzite polytype usually has a larger E0 gap than the zinc-blende polytype (Tables 6.1 and 6.2). Thus, the E0 value for w-MgSe should be larger than that for c-MgSe (4.0 eV). The solid line in Figure 6.56(d) shows the linearly interpolated result assuming E0 ¼ 4.1 eV for w-MgSe. The E0 versus x data for c-MgxCd1xSe layers (x 0.32) grown on InAs(100) have been determined using low-temperature (77 K) PL [319]. The bowing parameter c 0.2 eV is estimated from this study. The inset in Figure 6.56(d) shows the E0 versus x dependence at 300 K for c-MgxCd1xSe obtained by introducing c ¼ 0.200 eV into Equation (A.5) (see also Table 6.30). The composition dependence of E0 at 11 K for w-MgxCd1xSe has been determined from PL measurements [320]. The temperature dependence of E0 has also been reported by several authors [318,321]. Using SE, Wronkowska et al. [316] determined the higher-lying CPs for w-MgxCd1xSe. However, they explained these data using the notations of the zinc-blende lattice (E0 þ D0 and E1), not those of the wurtzite lattice (E0a and E1a (a ¼ A, B or C); see Adachi [1]). (e) ZnCdSe ZnxCd1xSe is commonly used as QW material in ZnSe-based devices. In the bulk form, ZnxCd1xSe has the zinc-blende structure at 0.7 x 1.0, the wurtzite structure at 0 x 0.3 and their mixed phases at 0.3 x 0.7 [322]. On the other hand, MBE-grown ZnxCd1xSe layers on GaAs(100) result in films of the zinc-blende structure over the whole composition range. The E0 versus x data for c-ZnxCd1xSe/GaAs(100) epilayers grown by MBE are shown in Figure 6.56(e) [323–326]. The solid line shows the quadratic least-squares fit of these data (see also Table 6.30). The higher-lying CPs in c-ZnxCd1xSe epilayers at 0 x 1.0 have been studied using SE in the 1.5–6.0 eV range [324]. The E0 þ D0, E1 and E1 þ D1 CPs have been observed and found to increase with increasing x. The corresponding bowing parameters are found to be c ¼ 0.38 (E0 þ D0), 0.467 (E1) and 0.351 eV (E1 þ D1). The temperature dependence of E0 for c-ZnxCd1xSe layers grown by MBE has been determined by several authors [326–328]. Using SE, Lee et al. [326] obtained an expression that allows E0 to be obtained for any composition and temperature within the ranges 0 x 0.34 and 25 T 260 C. The E0 versus T variation has also been determined by ER in the range 25 T 400 K for x ¼ 0.56 [327] and by PL in the range 15 T 250 K for 0 x 1.0 [328]. (f) CdHgSe CdxHg1xSe crystallizes in the zinc-blende structure at 0 < x < 0.77 and in the wurtzite structure at x > 0.81, while a mixed phase of both structures is observed at 0.77 < x < 0.81 [329]. The composition dependence of E0 for CdxHg1xSe is shown in Figure 6.56(f). The experimental data in the zinc-blende region are taken from Summers and Broerman [330] (solid circle), and those in the wurtzite region are taken from Himei and Muto [331] (open circles) and Pujari et al. [332] (open triangles). The E0 versus x data in the zinc-blende region can be satisfactorily approximated by the linear expression. The corresponding slope dE0/dx is given by 1.57 eV, as listed in Table 6.30. The experimental data in the wurtzite region differ largely among the literature, but clearly show nonlinear dependence on x.

204

PROPERTIES OF SEMICONDUCTOR ALLOYS

The interband CPs in CdxHg1xSe have been determined using reflectance spectroscopy for x up to 0.79 [333] and SE for 0 x 0.30 [334]. The E1 and E1 þ D1 CPs are found to linearly increase with increasing x up to 0.4 [333,334] and show an abrupt increase for x above 0.4 [333]. The temperature dependence of E0 for c-CdxHg1xSe has been studied by Summers and Broerman [330]. These results are shown in Figure 6.57(a). The experimental data suggest that the alloys at x < 0.7 have positive temperature coefficients. The solid line represents the dE0/dT versus x plots obtained from the linear interpolation between the HgSe ( þ 7.4 104 eV/K) and w-CdSe values (3.63 104 eV/K) [1]. It can be seen that the linear interpolation scheme explains the experimental data very well. 10 6 2

0

-2 (a) CdxHg1-xSe

-6 -10 dE0 / dT(10-4 eV/ K)

10 6 2

0

-2 -6

(b) ZnxHg1-xTe

-10 10 6 2

0

-2 -6 -10

(c) CdxHg1-xTe 0

0. 2

0. 4

0. 6

0. 8

1. 0

x

Figure 6.57 Temperature coefficient dE0/dT as a function of x for (a) CdxHg1xSe, (b) ZnxHg1xTe and (c) CdxHg1xTe. The experimental data are taken for (a) from Summers and Broerman [330] (solid circles), for (b) from Toulouse et al. [360] (solid circles) and for (c) from Hansen et al. [372] (solid line). The solid line in (a) represents the linearly interpolated values between the endpoint binary data taken from Adachi [1] (open squares). The solid line in (b) shows the linear least-squares fit of Equation (6.28)

6.5.4 (II, II)–Te Ternary Alloy (a) BeZnTe BexZn1xTe is a promising material for use as a p-type contact layer in various MgZnCdSebased devices. The composition dependence of E0 for c-BexZn1xTe is shown in Figure 6.58(a). The experimental data are taken from various sources [335–338]. The samples used were grown on InP(100) by MBE [335–337] or from the melt using the high-pressure Bridgman

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS 4.5

3.5

4 (b) Mg xZn1-xTe

(a) BexZn1-xTe

205

(c) MgxCd1-xTe

E0,E gX (eV)

4.0 zinc-blende

3.0

3.5

EgX

3.0 2.5

3

2.5 E0

EgX

X

Eg

E0

2

zinc-blende

E0

zinc-blende

E0 (eV)

2.0 2.0 1 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x 2.4 2.5 2.0 (d) Zn xCd1-xTe (e) ZnxHg1-xTe (f) CdxHg1-x Te 2.0 2.2 1.5 1.5

2.0

zinc-blende

zinc-blende

1.0

1.0 1.8

0.5

0.5

1.6

0

0 zinc-blende

semimetallic

semimetallic

1.4 -0.5 -0.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 x x x

Figure 6.58 Energy of the E0 gap versus x for some (II, II)Te ternaries at 300 K: (a) BexZn1xTe, (b) MgxZn1xTe, (b) MgxCd1xTe, (c) ZnxCd1xTe, (d) ZnxHg1xTe and (e) CdxHg1xTe. (f) The solid lines represent the calculated results using the data in Table 6.30. The dashed lines in (a)–(c) show the x dependence of EgX obtained by the linear interpolation between the endpoint binary data in Table 6.1. The gray lines in (d) represent the E0 versus x curves calculated using the experimental c values listed in Table 6.31. The heavy dashed line in (d) shows the E0 versus x curve calculated from the average c value of 0.27 eV

method [338]. These data suggest that the E0 gap is almost linearly dependent upon Be content x. Indeed, the least-squares fit of these data can be described by E0(x) ¼ 2.27 þ 1.83x eV (solid line, see also Table 6.30). The dashed line in Figure 6.58(a) shows the x dependence of EgX for cBexZn1xTe obtained by the linear interpolation between the ZnTe (x ¼ 0) and BeTe values (x ¼ 1.0) in Table 6.1. The G–X crossover is expected to occur at x 0.35 (E0 ¼ EgX 2.9 eV) for c-BexZn1xTe. The composition dependence of the higher-lying CPs, E0 þ D0, E1, E1 þ D1 and E2, for cBexZn1xTe has been determined using SE [336,337]. The E0 þ D0, E1 and E1 þ D1 CP energies increase at a rate of 0.8x eV, while E2 is found to increase at a lower rate of 0.2x eV. It is interesting to note the absence of bowing in any of the CPs. This is in contrast to most of the II–VI ternary alloys, such as BexZn1xSe [303] and ZnxCd1xSe [324], which all exhibit some degree of bowing about the CP energies. (b) MgZnTe MgxZn1xTecrystallizesinthezinc-blendestructureat0 x 0.53andinthewurtzitestructureat x 0.53 [339]. The E0 versus x data for c-MgxZn1xTe determined by wavelength-modulation

206

PROPERTIES OF SEMICONDUCTOR ALLOYS

(open circles) [340] and optical absorption spectroscopy (solid circle) are shown in Figure 6.58 (b) [341]. All samples used were grown by the Bridgman method. The solid line in Figure 6.58(b) shows the quadratic least-squares fit of these and c-MgTe (x ¼ 1.0) data, providing a value of c 0.46 eV. The dashed line in Figure 6.58(b) shows the x dependence of EgX for c-MgxZn1xTe obtained by the linear interpolation between ZnTe (x ¼ 0) and MgTe (x ¼ 1.0) as shown in Table 6.1. This result predicts the G–X crossover to occur at x 0.5 (E0 ¼ EgX 2.75 eV) for c-MgxZn1xTe. The higher-lying CPs in c-MgxZn1xTe have been studied using SE by Franz et al. [342]. The samples were grown by MBE on GaAs(100) substrates (0 x 0.52). The experimental data obtained by these authors show that the E1 and E1 þ D1 CPs increase almost linearly with increasing x, while a clear decrease in E2 is observed from x ¼ 0 (5.25 eV) to 0.52 (5.0 eV). The temperature variation of E0 for c-MgxZn1xTe has been measured by Barbier et al. [340] and Chung et al. [341]. The dE0/dT values near 300 K are given as (4.5 0.3) 104 (0 x 0.41) [340] and (5.9 0.2) 104 (0 x 0.48) eV/K [341], respectively, and are nearly independent of x. (c) MgCdTe Bulk MgxCd1xTe alloy crystallizes in the zinc-blende structure at 0 x 0.6 and in the wurtzite structure at x 0.75 [343]. The E0 versus x data for c-MgxCd1xTe are plotted in Figure 6.58(c) [344–346]. The samples were grown by the Bridgman method [345] or by MBE on ZnCdTe [344] and GaAs substrates [346]. The solid line represents the quadratic leastsquares fit of these and the c-MgTe (x ¼ 1.0) data. This fit results in a bowing of c 0.54 eV. The composition dependence of EgX for c-MgxCd1xTe obtained from the linear interpolation scheme between CdTe (x ¼ 0) and MgTe (x ¼ 1.0) in Table 6.1 is shown in Figure 6.58(c) by the dashed line. It can be seen that the G–X crossover occurs at x 0.7 with E0 ¼ EgX 2.8 eV, in good agreement with the theoretical prediction by Freytag [347]. The higher-lying CPs in c-MgxCd1xTe have been measured using SE by Choi et al. [345] at 0 x 0.5 and by Ihn et al. [346] at 0 x 0.43. These studies observed the E0 þ D0, E1, E1 þ D1, E2 and E10 CPs. Some CPs, E0 þ D0, E1 and E1 þ D1, increased almost linearly at a rate of (0.7 1.3)x eV, while E2 and E10 showed little dependence on x. (d) ZnCdTe ZnxCd1xTe crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. The dependence of E0 on x for ZnxCd1xTe has been determined by many authors. An overview of the bowing parameter c determined at 300 K is summarized in Table 6.31 and in Figure 6.58(d). The c values in Table 6.31 vary from 0 to 0.48 eV. The average c value is 0.27 eV. The corresponding E0 versus x plots are shown in Figure 6.58(d) by the heavy dashed line (see also Table 6.30). The higher-lying CPs, such as E1, E1 þ D1 and E2, in ZnxCd1xTe have been studied by many authors. These CPs showed no or a very weak nonlinearity with respect to x [348–354]. Several studies, however, reported a clear nonlinearity with respect to x [355,356]. The temperature dependence of E0 for ZnxCd1xTe has been studied using PR [357,358], reflectivity and PL [359]. The Varshni parameters have been determined as a ¼ (4.7 0.1) 104 eV/K and b ¼ 166.5 6.5 K for 0 x 0.3 [357] and a ¼ (4.7 0.2) 104 eV/K and

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

207

Table 6.31 Bowing parameter c for E0 of ZnxCd1xTe determined at 300 K. R ¼ reflectance; ER ¼ Electroreflectance; PL ¼ photoluminescence; OA ¼ optical absorption; PR ¼ photoreflectance; SE ¼ spectroscopic ellipsometry c (eV)

Method

Reference

0.33 0.26 0 0.139 0.22890 0.38 0.11 0.128 0.46 0.269 0.48 0.3156 0.334 0.33 0.197 0.33

R ER R PL OA OA PL PR OA SE OA OA PR R SE PR

a b c d e f g h i j k l m n o p

A. Ebina et al., J. Appl. Phys. 44, 3659 (1973) V. A. Tyagai et al., Sov. Phys. Solid State16, 885 (1974) c V. V. Sobolev et al., Phys. Status Solidi B 103, 499 (1981) d D. J. Olego et al., Appl. Phys. Lett. 47, 1172 (1985) e S. M. Johnson et al., J. Vac. Sci. Technol. B 9, 1897 (1991) f A. Aydinli et al., Solid State Commun. 80, 465 (1991) g H. C. Poon et al., J. Phys.: Condens. Matter 7, 2783 (1995) h S. P. Tobin et al., J. Electron. Mater. 24, 697 (1995) i B. Samanta et al., Vacuum 46, 739 (1995) j O. Castaing et al., J. Phys.: Condens. Matter 8, 5757 (1996) k D. Ohlmann et al., J. Appl. Phys. 82, 1355 (1997) l J. Franc et al., Semicond. Sci. Technol. 15, 561 (2000) m L. Tirado-Mejıa et al., Phys. Status Solidi B 220, 255 (2000) n E. M. Larramendi et al., Semicond. Sci. Technol. 17, 8 (2002) o P. D. Paulson et al., J. Appl. Phys. 95, 3010 (2004) p O. Zelaya-Angel et al., J. Appl. Phys. 95, 6284 (2004) a b

b ¼ 110 30 K for 0.551 x 0.944[359].These parameters provide dE0/dT 4 104 eV/ K near 300 K. The corresponding endpoint data are 4.53 104 eV/K (ZnTe) and 3.5 104 eV/K (CdTe) [1]. (e) ZnHgTe ZnxHg1xTe crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. The E0 versus x data for ZnxHg1xTe determined by means of optical absorption [360,361] and SE [361,362] are shown in Figure 6.58(e). The samples used were grown by the THM [360,362,363] or from interdiffusion between the endpoint materials at high temperatures [361]. The quadratic least-squares fit of these data is shown in Figure 6.58(e)

208

PROPERTIES OF SEMICONDUCTOR ALLOYS

by the solid line. The bowing parameter of c 0.46 eV can be determined from this fit (see also Table 6.30). The semimetallic region is in the range x < 0.08 at 300 K. The higher-lying CPs, E0 þ D0, E1, E1 þ D1 and E2, as a function of x for ZnxHg1xTe have been determined using SE [363]. The bowing parameters obtained are c ¼ 0.860 eV (E0 þ D0), 1.012 eV (E1), 0.817 eV (E1 þ D1) and 0.428 eV (E2). The temperature dependence of E0 for ZnxHg1xTe has been investigated by Toulouse et al. [360]. The results obtained are plotted in Figure 6.57(b). It can be seen that the alloy at x < 0.45 has a positive temperature coefficient. The solid line shows the linear least-squares fit given by (in 104 eV/K) dE0 ¼ 4:510:6x dT

ð6:28Þ

(f) CdHgTe CdxHg1xTe crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. Figure 6.58(f) plots the experimental E0 versus x data for CdxHg1xTe measured by Sredin et al. [364] (open circles), Laurenti et al. [365] (solid circles) and Chu et al. [366] (open triangles). The solid line shows the quadratic least-squares fit of these experimental data. The resulting bowing parameter is c 0.21 eV (Table 6.30). The semimetallic region is expected at x < 0.1 and 300 K. The higher-lying CPs, such as E1, E1 þ D1 and E2, as a function of x for CdxHg1xTe have been studied by fundamental reflectivity [364,367], ER [368] and SE [369,370]. They appeared at energies 2–3 (E1), 3–4 (E1 þ D1) and 4.5–5 eV (E2) and gradually increased with increasing x. The bowing parameters determined were c 0.7 0.9 eV for E1 and 0.5 0.6 eV for E1 þ D1 [369]. The c value for E2 was found to be negligibly small (c ¼ 0.06 eV). The temperature dependence of E0 for CdxHg1xTe has been studied by several authors [365,366,371,372]. The result obtained by Hansen et al. [372] is shown in Figure 6.57 (c). The sign for dE0/dT is positive at x < 0.5 and negative at x > 0.5. No temperature change in E0 can be expected at x 0.5 (E0 0.6 eV, Figure 6.58(f)). The dE0/dT value can then be given by (in 104 eV/K) dE0 ¼ 5:511:0x dT

ð6:29Þ

The temperature coefficients of the higher-lying CPs have been measured by several authors [367,373,374]. A dip in the dEg/dT versus x data has been observed near x 0.5 for E1, E1 þ D1, e1 and e1 þ D1 [367]. The E1-gap Varshni parameters a and b have also been determined using ER [373].

6.5.5 Zn–(VI, VI) Ternary Alloy (a) ZnOS ZnOxS1x is one of the II–VI large size-mismatched alloys and may thus behave in a similar manner to GaNx As1x [375]. The E0 gap as a function of x for ZnOxS1x has been determined from transmission measurements by Meyer et al. [376]. The alloy films (0 x 1.0) used were

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

209

grown by rf reactive sputtering on glass and (0001)-sapphire substrates and showed wurtzite structure with preferential c-axis orientation independent of whether glass or sapphire substrates were used. Figure 6.59(a) plots the E0 versus x data measured by Meyer et al. [376]. The solid line shows the quadratic fit of these data and results in a huge bowing parameter of c ¼ 4.50 eV (Table 6.30). This is in qualitative agreement with the fact that bowing parameters in large size-mismatched II–VI alloys increase as the size and chemical mismatches between the endpoint constituents increase [375]. 4.0

4.0 (a) ZnOxS1-x

3.5

4.0 (b) ZnSxSe1-x

3.5

4.0 (c) ZnSxTe1-x

3.5

(d) ZnSexTe1-x

3.5

E0 (eV)

zinc-blende

zinc-blende

3.0

3.0

3.0

3.0

2.5

2.5

2.5

2.5

2.0

2.0

2.0

2.0 wurtzite

zinc-blende

1.5 1.5 1.5 1.5 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0 0 0.2 0.4 0.6 0.8 1.0

x

x

x

x

Figure 6.59 Energy of the E0 gap versus x for some Zn–(VI, VI) ternaries at 300 K: (a) ZnOxS1x, (b) ZnSxSe1x, (c) ZnSxTe1x and (d) ZnSexTe1x. The solid lines represent the calculated results using the data in Table 6.30

(b) ZnOSe ZnOxSe1x at x ¼ 0.35 1.3 at% has been successfully grown on GaAs(100) by MBE in spite of the limited solubility of oxygen in ZnSe [377]. A large bowing parameter, as high as 8 eV has been obtained [377] and a reduced pressure coefficient has been successfully explained within the framework of the BAC model [378]. More recently, the temperature variation of E0 in ZnOxSe1x (x ¼ 0.23 0.90 at%) before and after hydrogen passivation was found to be similar to that for ZnSe and did not depend on the oxygen concentration [379]. Such a finding points toward the absence of a localized character in the ZnOxSe1x band edge. (c) ZnSSe c-ZnSxSe1x can be grown from the melt throughout the whole composition range 0 x 1.0, although the alloy at x 0.9 sometimes shows a short-range twin structure which is typically observed in ZnS grown from the melt [380]. We show in Figure 6.59(b) the x dependence of E0 in ZnSxSe1x determined by fundamental reflectivity [380] (solid circles), CL [381] (open circles) and optical absorption measurements [382] (open triangles). The solid line shows the quadratic least-squares fit of these data. The resulting bowing parameter is c ¼ 0.580 eV (Table 6.30). The low-temperature (T 6 K) E0 versus x data for ZnSxSe1x have also been reported [381,383]. The pressure coefficient dE0/ dp for p up to 12 GPa has been measured by Griebl et al. [382].

210

PROPERTIES OF SEMICONDUCTOR ALLOYS

(d) ZnSTe ZnSxTe1x is one of the II–VI large size-mismatched alloys and may have a large bowing of the E0 gap. The E0 versus x data reported by Hill and Richardson [384] (solid circles), Yu et al. [385] (open circles) and by Walukiewicz et al. [386] (open triangles) are shown in Figure 6.59(c). The samples were grown by vacuum evaporation [384], hot-wall epitaxy [385] or by the Bridgman method [386]. The solid line in Figure 6.59(c) shows the quadratic least-squares fit of the data of Yu et al. and Walukiewicz et al. The resulting bowing parameter is c ¼ 3.750 eV (Table 6.30). The data of Hill and Richardson gave a value of c 3.0 eV [384]. SE has been used by Bang et al. [387] on ZnSxTe1x epilayers (0 x 1.0) grown on GaAs (100) substrates by hot-wall epitaxy. The E0 þ D0 and E1 structures merged into a single, broad structure for x larger than 0.3. The pressure dependence of E0 in ZnSxTe1x (x ¼ 0–0.1) has been studied by Walukiewicz et al. [386] (x ¼ 0–0.1) for p up to 10 GPa. A strong nonlinear dependence of E0 on p was observed by optical absorption measurements. The results can be satisfactorily described by the BAC model. (e) ZnSeTe ZnSexTe1x crystallizes in the zinc-blende structure over the whole composition range 0 x 1.0. The composition dependence of E0 has been studied by several authors. The E0 versus x data measured by Larach et al. [388] (solid circles), Ebina et al. [389] (open circles), Brasil et al. [390] (solid triangles) and Su et al. [391] (open triangles) have been plotted in Figure 6.59(d) The quadratic least-squares fit of these data is shown by the solid line. The bowing parameter obtained is c ¼ 1.500 eV (Table 6.30). This value is considerably larger than that for ZnSxSe1x (c ¼ 0.580 eV, Figure 6.59(b)), but is much smaller than those for ZnOxS1x (c ¼ 4.50 eV, Figure 6.59(a)) and ZnSxTe1x (c ¼ 3.750 eV, Figure 6.59(c)). The higher-lying CPs, such as E0 þ D0, E1, E1 þ D1 and E2, as a function of x for ZnSexTe1x have been measured by fundamental reflectivity [389] and SE [392]. The bowing parameters determined were c ¼ 1.878 eV (E1), 1.458 eV (E1 þ D1) and 0.698 eV (E2) [392]. Only the E2 CP gives an upward bowing (c < 0 eV). The high-energy PL line as a function of temperature T for ZnSexTe1x (0 x 0.30) has been measured by Naumov et al. [393]. The experimental data could be fitted with the Varshni expression using the interpolated parameters between ZnTe (x ¼ 0) and ZnSe (x ¼ 1.0) [1]. The pressure dependence of E0 has also been measured for p up to 10 GPa [394]. The first- and second-order pressure coefficients are reported as a function of x for 0 x 1.0. The large deviation of dE0/dp from the linear interpolation can be explained by the BAC model [394].

6.5.6 Cd–(VI, VI) Ternary Alloy (a) CdSSe CdSxSe1x crystallizes in the wurtzite structure over the whole composition range 0 x 1.0. The experimental E0 value as a function of x for w-CdSxSe1x measured by Bondarenko et al. [395] (solid circles) and Perna et al. [396] are shown in Figure 6.60(a). The quadratic fit of these data gives a value of c ¼ 0.700 eV (Table 6.30).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

211

The higher-lying CPs, such as E1, E2 and E10, in w-CdSxSe1x have been determined from the fundamental reflectivity measurements for the ordinary (E ? c) and extraordinary rays (E||c) at 90 K [397]. The temperature dependence of E0 in w-CdSxSe1x has been studied by Perna et al. [396]. These authors reported that the effects of the acoustic phonons are larger in alloy films than in the related binaries because of the compositional disorder. (b) CdSTe The CdS–CdTe phase diagram indicates that at low temperatures, CdSxTe1x has a zinc-blende structure for low S concentrations and a wurtzite structure for high S concentrations (Figure 2.7). These regions are separated by a miscibility gap where both phases exist, and optical transitions resulted from both wide band-gap wurtzite and narrow band-gap zinc-blende phases. Therefore, the two absorption edges would usually be detected, although their strengths would depend on the concentration of each phase. Many authors have measured the E0 versus x data for CdSxTe1x films (see Lane [398]). A small number of samples of different x have been studied generally, with the most widely accepted results relying on 19 data points from x ¼ 0 to 1.0 reported by Ohata et al. [399]. From the quadratic fit of the previous data, we obtain a bowing parameter of c 1.8 eV for both the zinc-blende and wurtzite phases (see also Figure 1 in Lane [398] and Figure 6.63). The curves plotted in Figure 6.60(b) show the quadratic fits of Equation (A.5) with c 1.8 eV (Table 6.30). 3.00

2.6

(a) CdSxSe1-x 2.75

1.8

(b) CdSxTe1-x 2.4

(c) CdSexTe1-x 1.7

miscibility gap

E0 (eV)

2.50

wurtzite

2.2

zinc-blende

1.6 zinc-blende

2.25

2.0

2.00

1.8

wurtzite

1.5 1.4

wurtzite

1.75

1.6

1.3 zinc-blende

1.50

0 0.2 0.4 0.6 0.8 1.0 x

1.4

0 0.2 0.4 0.6 0.8 1.0 x

1.2

0 0.2 0.4 0.6 0.8 1.0 x

Figure 6.60 Energy of the E0 gap versus x for some Cd(VI, VI) ternaries at 300 K: (a) CdSxSe1x, (b) CdSxTe1x and (c) CdSexTe1x. The solid and dashed lines represent the calculated results using the data in Table 6.30

The higher-lying CPs in c-CdSxTe1x (x ¼ 0 1.0) have been determined using SE [400]. The samples used were deposited on borosilicate glass (Corning 7059) using a laser-deposition process. The XRD analysis suggested that the deposited films consisted of a single phase. The bowing parameter determined for the E1 gap is c 0.8 eV, while that for E0 is 1.84 eV. (c) CdSeTe Since CdSe is a wurtzite crystal while CdTe is a zinc-blende crystal, it is reasonable to expect a phase change in crystal structure at some Se composition. This has been reported for alloys

212

PROPERTIES OF SEMICONDUCTOR ALLOYS

grown on glass substrates with zinc-blende nucleation at x < 0.60 and wurtzite nucleation at x > 0.60 [401]. Similarly, melt-grown CdSexTe1x was reported to nucleate as zinc-blende at x 0.45 and as wurtzite at x 0.65 with a mixed phase between x ¼ 0.45 and 0.65 [402]. Figure 6.60(c) shows the plots of E0 against x for c-CdSexTe1x reported by Feng et al. [403] (solid circles) and Brill et al. [404] (open circles). The samples were grown by the Bridgman method (x < 0.36) [403] and by MBE on Si(211) (0 x 1.0) [404]. It could be clearly observed that the MBE-grown CdSexTe1x/Si(211) films remained in the cubic phase throughout the entire composition range [404]. Note that CdSe can be grown in the cubic phase on GaAs and ZnSe substrates (see Brill et al. [404]). The solid line in Figure 6.60(c) represents the quadratic least-squares fit of the experimental data, yielding a value of c ¼ 0.838 eV (Table 6.30).

6.5.7 (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe MgxZn1xSySe1y can be grown lattice-matched to GaAs (Table 1.13) and has been used as an improved cladding material for ZnSe-based waveguiding devices [405]. The E0-gap energy as a function of x for MgxZn1xSySe1y/GaAs calculated from Equation (A.15) is shown in Figure 6.61(a).The experimental data shown are taken from Lunz et al. [406]

5.0

4.0

5.0

3.5

(a) MgxZn1-xSySe1-y /GaAs 4.5

3.0

4.5

2.5 2.0 0

4.0 E0 (eV)

E0 (eV)

4.0 3.5

on ZnTe

0.5

1.0

3.5

3.0

3.0

2.5

2.5

2.0

2.0

(b) MgxZn1-xSeyTe1-y /InP 0

0.2

0.4

0.6 x

0.8

1.0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 6.61 Energy of the E0 gap versus x for (a) MgxZn1xSySe1y/GaAs and (b) MgxZn1x

SeyTe1y/InP calculated from Equation (A.15). The ternary bowing parameters are taken from Table 6.32. The unknown ternary and quaternary bowing parameters (c and D) are assigned to be 0 eV. The experimental data in (a) are taken from Lunz et al. [406] (solid circles) and Chen et al. [407] (open circle) and in (b) from Naniwae et al. [408] (300 K). The dashed line in (a) shows the quadratic approximation of Equation (A.15) for 0 x 0.5 (see Table 6.30). The inset in (b) represents the E0 versus x data for MBE-grown MgxZn1xSeyTe1y/ZnTe reported by Shim et al. [409]. The solid line in the inset is calculated from Equation (6.30)

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

213

(solid circles) and Chen et al. [407] (open circle). It can be seen that the calculated E0 varies from 2.749 eV (x ¼ 0, y ¼ 0.06) to 4.399 eV (x ¼ 1.00, y ¼ 0.89). This curve can be approximated by the quadratic expression as shown in Figure 6.61(a) by the dashed line (Table 6.30). The temperature dependence of E0 for MgxZn1xSySe1y/GaAs has been determined by Lunz et al. [406] from an optical absorption and by Chen et al. [407] from contactless ER. The dE0/dT coefficient near 300 K is 6 104 eV/K, while that for ZnSe is 4.7 104 eV/ K [1]. (b) MgZnSeTe MgxZn1xSeyTe1y can be grown lattice-matched to InP (Table 1.13). The solid line in Figure 6.61(b) shows the E0 versus x curve for MgxZn1xSeyTe1y/InP obtained from Equation (A.15). The solid circles represent the experimental data measured by optical reflectivity [408]. The solid line can be approximated by the quadratic expression given in Table 6.30. MgxZn1xSeyTe1y can be grown lattice-matched to ZnTe. Shim et al. [409] grew MgxZn1xSeyTe1y/ZnTe by MBE and determined E0 from PL measurements. The inset in Figure 6.61(b) shows the E0 versus x data of Shim et al. [409]. These data can be least-squares fit as (in eV) E0 ðxÞ ¼ 2:36 þ 0:89x þ 0:82x2

ð6:30Þ

6.5.8 (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe BexMgyZn1xySe can be grown lattice-matched to GaAs (Table 1.14). The experimental E0 versus y data for BexMgyZn1xySe/GaAs are plotted in Figure 6.62(a). These data are taken from Wagner et al. [410] (solid circles) and Godo et al. [411] (open circles). The solid line represents the E0 versus y curve for BexMgyZn1xySe/GaAs calculated from Equation (A.15). This curve can be satisfactorily approximated by the quadratic expression shown in Table 6.30. The E0/(E0 þ D0) structure of Bridgman-grown BexMgyZn1xySe alloy (x ¼ 0.04, y ¼ 0.15) has been investigated by PL, contactless ER and PR in the temperature range between 15 and 400 K [412]. The obtained data were analyzed using the Varshni and Bose–Einstein expressions. (b) BeZnCdSe Bulk BexZnyCd1xySe alloys were grown by the Bridgman method and investigated using ER, PR, SE and PL [413–415]. The samples were single wurtzite phase or wurtzite as the main phase in an admixture with another polytype (x 0.15, y 0.45). The temperature dependence of E0 has been reported [413,415]. BexZnyCd1xySe can be epitaxially grown lattice-matched to InP. Hsieh et al. [416] have characterized the E0 structure of MBE-grown BexZnyCd1xySe/InP using contactless ER and PzR in the temperature range between 15 and 450 K. The results show that Be incorporation can effectively reduce the rate of temperature variation of E0.

214

PROPERTIES OF SEMICONDUCTOR ALLOYS 5.0

4.0

(a) Bex Mgy Zn1-x-y Se/GaAs

(b) Mg x Zny Cd 1-x-y Se/InP

4.5 3.5 E0 (eV)

E0 (eV)

4.0 3.5

3.0

3.0 2.5 2.5 2.0

0

0.2

0.4

0.6

0.8

1.0

2.0

0

0.2

y

0.4

0.6

0.8

1.0

x

Figure 6.62 Energy of the E0 gap versus y or x for (a) BexMgyZn1xySe/GaAs and (b)

MgxZnyCd1xySe/InP calculated from Equation (A.15). The ternary bowing parameters are taken from Table 6.32 (see also Table 6.30). The unknown ternary and quaternary bowing parameters (c and D) are assigned to be 0 eV. The experimental data in (a) are taken from Wagner et al. [410] (solid circles) and Godo et al. [411] (open circles) (300 K). The solid circles in (b) are obtained from Maksimov et al. [417]. The solid lines show the quadratic approximations listed in Table 6.30 (c) MgZnCdSe MgxZnyCd1xySe can be grown, together with those for the E0 and E0 þ D0 CPs latticematched to InP (Table 1.14). Figure 6.62(b) plots the E0 versus x data for MgxZnyCd1xySe/ InP measured by Maksimov et al. [417]. The E0 versus x curve calculated from Equation (A.15) is shown by the solid line. The corresponding quadratic expression is given in Table 6.30. The temperature dependence of E0 has also been determined by Maksimov et al. [417] in the temperature range between 4.2 and 300 K.

6.5.9 Summary Table 6.32 summarizes the bowing parameter c for E0 in some II–VI ternary alloys. Figure 6.63 also shows the plots for the c value against the product DaabDXab of the lattice constant and electronegativity differences between the endpoint binaries a and b. The electronegativity differences are obtained from Phillips [46]. The solid line in Figure 6.63 represents the leastsquares fit obtained using the relationship (c in eV, DaabDXab in AeV) c ¼ 6:13ðDaab DXab Þ

ð6:31Þ

Note that the proportionality factor 6.13 A1 obtained here is considerably smaller than the 1 values 9.93 and 9.62 A for the group-IV binary and III–V ternary alloys, respectively (Equations (6.8) and (6.23)). Finally, the relationships between the E0 gap and lattice constant a0 for various II–VI semiconductors are shown in Figure 6.64. It is clear that the lowest direct gap E0 can be widely

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

215

Table 6.32 Bowing parameter c for E0 in II–VI ternaries. w ¼ wurtzite; zb ¼ zinc-blende (II, II)–VI

c (eV)

II–(VI, VI)

c (eV)

BeZnO (w) MgZnO (w) ZnCdO (w) MgZnS (zb) MgZnS (w) ZnCdS (zb) ZnCdS (w) ZnHgS (zb) CdHgS (w) BeZnSe (zb) BeCdSe (zb) MgZnSe (zb) MgCdSe (zb) MgCdSe (w) ZnCdSe (zb) CdHgSe (zb) BeZnTe (zb) MgZnTe (zb) MgCdTe (zb) ZnCdTe (zb) ZnHgTe (zb) CdHgTe (zb)

9.3 0 2.4 0 0 0.827 0.921 0.996 0 1.033 3.000 0.600 0.200 0 0.387 0 0 0.46 0.54 0.31 0.46 0.21

ZnOS (w) ZnSSe (zb) ZnSTe (zb) ZnSeTe (zb) CdSSe (w) CdSTe (zb) CdSTe (w) CdSeTe (zb)

4.50 0.580 3.750 1.500 0.700 1.80 1.800 0.838

6.0 5.0

c (eV)

4.0

ZST BCSe

3.0 CST

2.0

ZSeT ZHS

1.0

BZSe CSeT

0

0

0.20

0.40

0.60

0.80

1.00

∆aAB∆XAB (Å eV)

Figure 6.63 Bowing parameter c of the E0 gap versus product DaabDXab of the lattice-constant and electronegativity differences between the endpoint binary materials a and b in some II–VI semiconductor ternary alloys. The solid line represents the calculated result using Equation (6.31). B ¼ Be; Z ¼ Zn; C ¼ Cd; T ¼ Te

216

PROPERTIES OF SEMICONDUCTOR ALLOYS GaP GaAs

6

InP

InAs

InSb

BeSe 5

MgS BeTe

4

ZnS

MgTe

ZnSe

3

E0 (eV)

MgSe

CdS

ZnTe

2

CdSe

CdTe

1 0

HgS

Semimetallic -1 5.0

5.2

5.4

5.6

5.8

6.0

HgSe 6.2

HgTe 6.4

6.6

6.8

a (Å)

Figure 6.64 Relationships between the E0 gap and lattice constant a0 for II–VI semiconductor systems

varied by properly combining the binary materials when growing II–VI ternary and quaternary alloys. Such alloys can be epitaxially grown on commercially available III–V binary substrates, such as GaP, GaAs and InP.

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] J. L. Birman, Phys. Rev. 115, 1493 (1959). [3] D. G. Thomas and J. J. Hopfield Phys. Rev. 116, 573 (1959); J. J. Hopfield J. Phys. Chem. Solids 15, 97 (1960). [4] J. A. Van Vechten and T. K. Bergstresser, Phys. Rev. B 1, 3351 (1970). [5] J. C. Phillips and J. A. Van Vechten, Phys. Rev. Lett. 22, 705 (1969). [6] P. Kiesel, T. Kippenberg, and G. H. D€ohler, in Spontaneous Ordering in Semiconductor Alloys (edited by A. Mascarenhas), Kluwer Academic, New York, 2002, p. 365. [7] G. F. Koster, J. O. Dimmock, R. G. Wheeler, and H. Statz, Properties of Thirty-Two Point Groups, MIT Press, Cambridge, 1963. [8] P. Ernst, C. Geng, F. Scholz, H. Schweizer, Y. Zhang, and A. Mascarenhas, Appl. Phys. Lett. 67, 2347 (1995). [9] B. T. McDermott, K. G. Reid, N. A. El-Masry, S. M. Bedair, W. M. Duncan, X. Yin, and F. H. Pollak, Appl. Phys. Lett. 56, 1172 (1990). [10] R. L. Forrest, T. D. Golding, S. C. Moss, Z. Zhang, J. F. Geisz, J. M. Olson, A. Mascarenhas, P. Ernst, and C. Geng, Phys. Rev. B 58, 15355 (1998). [11] W. Kissinger, M. Weidner, H. J. Osten, and M. Eichler, Appl. Phys. Lett. 65, 3356 (1994). [12] S. Zollner, C. M. Herzinger, J. A. Woollam, S. S. Iyer, A. P. Powell, and K. Eberl, Solid State Commun. 96, 305 (1995). [13] A. A. Demkov and O. F. Sankey, Phys. Rev. B 48, 2207 (1993).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

217

[14] H. Lee, S. R. Kurtz, J. A. Floro, J. Strane, C. H. Seager, S. R. Lee, E. D. Jones, J. F. Nelson, T. Mayer, and S. T. Picraux, Jpn. J. Appl. Phys. 34, L1340 (1995). [15] S. Zollner, K. E. Junge, R. Lange, and A. A. Affolder, Jpn. J. Appl. Phys. 35, 5684 (1996). [16] J. Kolodzey, P. A. O’Neil, S. Zhang, B. A. Orner, K. Roe, K. M. Unruh, C. P. Swann, M. M. Waite, and S. I. Shah, Appl. Phys. Lett. 67, 1865 (1995). [17] J. S. Schrader, J. L. Huguenin-Love, R. J. Soukup, N. J. Ianno, C. L. Exstrom, S. A. Darveau, R. N. Udey, and V. L. Dalal, Sol. Ener. Mater. Sol. Cells 90, 2338 (2006). [18] K. E. Junge, N. R. Voss, R. Lange, J. M. Dolan, S. Zollner, M. Dashiell, D. A. Hits, B. A. Orner, R. Jonczyk, and J. Kolodzey, Thin Solid Films 313–314, 172 (1998). [19] See, for example, Semiconductors and Semimetals (edited by R. K. Willardson and A. C. Beer), Academic, New York, 1991, Vol. 33 (Volume Editor, T. P. Pearsall). [20] R. Braunstein, A. R. Moore, and F. Herman, Phys. Rev. 109, 695 (1958). [21] J. Weber and M. I. Alonso, Phys. Rev. B 40, 5683 (1989). [22] D. V. Lang, R. People, J. C. Bean, and A. M. Sergent, Appl. Phys. Lett. 47, 1333 (1985). [23] D. Dutartre, G. Bremond, A. Souifi, and T. Benyattou, Phys. Rev. B 44, 11525 (1991). [24] C. W. Liu, J. C. Sturm, Y. R. J. Lacroix, M. L. W. Thewalt, and D. D. Perovic, Appl. Phys. Lett. 65, 76 (1994). [25] R. People, Phys. Rev. B 32, 1405 (1985); 34, 2508 (1986). [26] F. Ferrieu, F. Beck, and D. Dutartre, Solid State Commun. 82, 427 (1992). [27] R. T. Carline, C. Pickering, D. J. Robbins, W. Y. Leong, A. D. Pitt, and A. G. Cullis, Appl. Phys. Lett. 64, 1114 (1994). [28] R. T. Carline, T. J. C. Hosea, and D. J. Hall, J. Appl. Phys. 78, 4285 (1995). [29] J. H. Bahng, K. J. Kim, S. H. Ihm, and J. Y. Kim, Solid State Commun. 106, 591 (1998). [30] T. Ebner, K. Thonke, R. Sauer, F. Schaeffler, and H. J. Herzog, Phys. Rev. B 57, 15448 (1998). [31] P. Etchegoin, J. Kircher, and M. Cardona, Phys. Rev. B 47, 10292 (1993). [32] J. Humlıcek, F. Lukes, E. Schmidt, M. G. Kekoua, and E. Khoutsishvili, Phys. Rev. B 33, 1092 (1986). [33] E. Schmidt and K. Vedam, Solid State Commun. 9, 1187 (1971). [34] G. He and H. A. Atwater, Phys. Rev. Lett. 79, 1937 (1997). [35] H. P. L. de Guevara, A. G. Rodrıguez, H. Navarro-Contreras, and M. A. Vidal, Appl. Phys. Lett. 84, 4532 (2004); 91, 161909 (2007). [36] M. R. Bauer, J. Tolle, C. Bungay, A. V. G. Chizmeshya, D. J. Smith, J. Menendez, and J. Kouvetakis, Solid State Commun. 127, 355 (2003). [37] V. R. D’Costa, C. S. Cook, A. G. Birdwell, C. L. Littler, M. Canonico, S. Zollner, J. Kouvetakis, and J. Menendez, Phys. Rev. B 73, 125207 (2006). [38] A. S. Amour, C. W. Liu, J. C. Sturm, Y. Lacroix, and M. L. W. Thewalt, Appl. Phys. Lett. 67, 3915 (1995). [39] C. G. Van de Walle and R. M. Martin, Phys. Rev. B 34, 5621 (1986). [40] O. G. Schmidt and K. Eberl, Phys. Rev. Lett. 80, 3396 (1998). [41] H. Lee, J. A. Floro, J. Strane, S. R. Lee, E. D. Jones, T. Mayer, and S. T. Picraux, Mater. Res. Soc. Symp. Proc. 379, 211 (1995). [42] W. Kissinger, H. J. Osten, M. Weidner, and M. Eichler, J. Appl. Phys. 79, 3016 (1996). [43] P. Aella, C. Cook, J. Tolle, S. Zollner, A. V. G. Chizmeshya, and J. Kouvetakis, Appl. Phys. Lett. 84, 888 (2004). [44] V. R. D’Costa, C. S. Cook, J. Menendez, J. Tolle, J. Kouvetakis, and S. Zollner, Solid State Commun. 138, 309 (2006). [45] R. A. Soref, J. Appl. Phys. 70, 2470 (1991). [46] J. C. Phillips, Bonds and Bands in Semiconductors, Academic, New York, 1973. [47] H. Okumura, T. Koizumi, Y. Ishida, H. Yaguchi, and S. Yoshida, Phys. Status Solidi B 216, 211 (1999). [48] T. Suzuki, H. Yaguchi, H. Okumura, Y. Ishida, and S. Yoshida, Jpn. J. Appl. Phys. 39, L497 (2000).

218

PROPERTIES OF SEMICONDUCTOR ALLOYS

[49] A. Kasic, M. Schubert, T. Frey, U. K€ohler, D. J. As, and C. M. Herzinger, Phys. Rev. B 65, 184302 (2002). [50] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [51] M. P. Thompson, G. W. Auner, T. S. Zheleva, K. A. Jones, S. J. Simko, and J. N. Hilfiker, J. Appl. Phys. 89, 3331 (2001). [52] D. Brunner, H. Angerer, E. Bustarret, F. Freudenberg, R. H€ opler, R. Dimitrov, O. Ambacher, and M. Stutzmann, J. Appl. Phys. Lett. 82, 5090 (1997). [53] J. F. Muth, J. D. Brown, M. A. L. Johnson, Z. Yu, R. M. Kolbas, J. W. Cook, Jr., and J. F. Schetzina, Mater. Res. Soc. Symp. Proc. 537, G5.2 (1999). [54] B. K. Meyer, G. Steude, A. G€oldner, A. Hoffmann, H. Amano, and I. Akasaki, Phys. Status Solidi B 216, 187 (1999). [55] C. Buchheim, R. Goldhahn, M. Rakel, C. Cobet, N. Esser, U. Rossow, D. Fuhrmann, and A. Hangleiter, Phys. Status Solidi B 242, 2610 (2005). [56] I. Vurgaftman and J. R. Meyer, J. Appl. Phys. 94, 3675 (2003). [57] J. Wu, W. Walukiewicz, K. M. Yu, J. W. Ager III, S. X. Li, E. E. Haller, H. Lu, and W. J. Schaff, Solid State Commun. 127, 411 (2003). [58] S. R. Lee, A. F. Wright, M. H. Crawford, G. A. Petersen, J. Han, and R. M. Biefeld, Appl. Phys. Lett. 74, 3344 (1999). [59] T. Wethkamp, K. Wilmers, N. Esser, W. Richter, O. Ambacher, H. Angerer, G. Jungk, R. L. Johnson, and M. Cardona, Thin Solid Films 313–314, 745 (1998). [60] W. Shan, J. W. Ager III, W. Walukiewicz, E. E. Haller, B. D. Little, J. J. Song, M. Schurman, Z. C. Feng, R. A. Stall, and B. Goldenberg, Appl. Phys. Lett. 72, 2274 (1998). [61] F. Yun, M. A. Reshchikov, L. He, T. King, and H. Morko˛c , J. Appl. Phys. 92, 4837 (2002). [62] L. Malikova, Y. S. Huang, F. H. Pollak, Z. C. Feng, M. Schurman, and R. A. Stall, Solid State Commun. 103, 273 (1997). [63] N. Nepal, J. Li, M. L. Nakarmi, J. Y. Lin, and H. X. Jiang, Appl. Phys. Lett. 87, 242104 (2005). [64] W. Shan, J. W. Ager III, K. M. Yu, W. Walukiewicz, E. E. Haller, M. C. Martin, W. R. McKinney, and W. Yang, J. Appl. Phys. 85, 8505 (1999). [65] J. Wu and W. Walukiewicz, Superlatt. Microstruct. 34, 63 (2003). [66] M. Androulidaki, N. T. Pelekanos, K. Tsagaraki, E. Dimakis, E. Iliopoulos, A. Adikimenakis, E. Bellet-Amalric, D. Jalabert, and A. Georgakilas, Phys. Status Solidi C 3, 1866 (2006). [67] W. Terashima, S.-B. Che, Y. Ishitani, and A. Yoshikawa, Jpn. J. Appl. Phys. 45, L539 (2006). [68] R. Goldhahn, P. Schley, A. T. Winzer, G. Gobsch, V. Cimalla, O. Ambacher, M. Rakel, C. Cobet, N. Esser, H. Lu, and W. J. Schaff, Phys. Status Solidi A 203, 42 (2006). [69] S. X. Li, J. Wu, E. E. Haller, W. Walukiewicz, W. Shan, H. Lu, and W. J. Schaff, Appl. Phys. Lett. 83, 4963 (2003). [70] J. Sch€ormann, D. J. As, K. Lischka, P. Schley, R. Goldhahn, S. F. Li, W. L€ offler, M. Hetterich, and H. Kalt, Appl. Phys.Lett. 89, 261903 (2006). [71] J. R. M€ullh€auser, O. Brandt, A. Trampert, B. Jenichen, and K. H. Ploog, Appl. Phys. Lett. 73, 1230 (1998). [72] R. Goldhahn, J. Scheiner, S. Schokhovets, T. Frey, U. K€ ohler, D. J. As, and K. Lischka, Appl. Phys. Lett. 76, 291 (2000). [73] C. A. Parker, J. C. Roberts, S. M. Bedair, M. J. Reed, S. X. Liu, N. A. El-Masry, and L. H. Robins, Appl. Phys. Lett. 75, 2566 (1999). [74] C. Caetano, L. K. Teles, M. Marques, A. Dal Pino, Jr., and L. G. Ferreira, Phys. Rev. B 74, 045215 (2006). [75] P. Schley, R. Goldhahn, A. T. Winzer, G. Gobsch, V. Cimalla, O. Ambacher, H. Lu, W. J. Schaff, M. Kurouchi, Y. Nanishi, M. Rakel, C. Cobet, and N. Esser, Phys. Rev. B 75, 205204 (2007). [76] K. M. Yu, Z. Liliental-Weber, W. Walukiewicz, W. Shan, J. W. Ager III, S. S. Li, R. E. Jones, E. E. Haller, H. Lu, and W. J. Schaff, Appl. Phys. Lett. 86, 071910 (2005).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

219

[77] W. Shan, B. D. Little, J. J. Song, Z. C. Feng, M. Schurman, and R. A. Stall, Appl. Phys. Lett. 69, 3315 (1996). [78] W. Shan, W. Walukiewicz, E. E. Haller, B. D. Little, J. J. Song, M. D. McCluskey, N. M. Johnson, Z. C. Feng, M. Schurman, and R. A. Stall, J. Appl. Phys. 84, 4452 (1998). [79] H. Sonomura, T. Nanmori, and T. Miyauchi, Appl. Phys. Lett. 24, 77 (1974). [80] A. Onton, M. R. Lorenz, J. M. Woodall, and R. J. Chicotka, J. Cryst. Growth 27, 166 (1974). [81] L. K. Vodop’yanov, V. I. Kozlovskiı, and N. N. Mel’nik, Sov. Phys. Semicond. 34, 405 (2000). [82] J. M. Rodrıguez and G. Armelles, J. Appl. Phys. 69, 965 (1991). [83] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, D. H. Woo, and S. H. Kim, J. Appl. Phys. 87, 1287 (2000). [84] A. Onton and R. J. Chicotka, J. Appl. Phys. 41, 4205 (1970). [85] D. P. Bour, J. R. Shealy, G. W. Wicks, and W. J. Schaff, Appl. Phys. Lett. 50, 615 (1987). [86] Y. Ishitani, H. Hamada, S. Minagawa, H. Yaguchi, and Y. Shiraki, Jpn. J. Appl. Phys. 36, 6607 (1997). [87] A. Onton, M. R. Lorenz, and W. Reuter, J. Appl. Phys. 42, 3420 (1971). [88] C. Alibert, G. Bordure, A. Laugier, and J. Chevallier, Phys. Rev. B 6, 1301 (1972). [89] I. Vurgaftman, J. R. Meyer, and L. R. Ram-Mohan, J. Appl. Phys. 89, 5815 (2001). [90] H. Lange, J. Donecker, and H. Friedrich, Phys. Status Solidi B 73, 633 (1976). [91] M. Bugajski, A. M. Kontkiewicz, and H. Mariette, Phys. Rev. B 28, 7105 (1983). [92] R. Hill, J. Phys. C: Solid State Phys. 7, 516 (1974). [93] H. Lee, D. Biswas, M. V. Klein, H. Morko˛c , D. E. Aspnes, B. D. Choe, J. Kim, and C. O. Griffiths, J. Appl. Phys. 75, 5040 (1994). [94] Y. Ishitani, H. Yaguchi, and Y. Shiraki, Jpn. J. Appl. Phys. 40, 1183 (2001). [95] Y. C. Yeh, S. Chen, Y. S. Huang, C. H. Ho, and K. K. Tiong, J. Phys.: Condens. Matter 12, 2183 (2000). [96] R. Ferrini, G. Guizzetti, M. Patrini, A. Parisini, L. Tarricone, and B. Valenti, Eur. Phys. J. B 27, 449 (2002). [97] A. Onton and R. J. Chicotka, Phys. Rev. B 4, 1847 (1971). [98] B. W. Hakki, A. Jayaraman, and C. K. Kim, J. Appl. Phys. 41, 5291 (1970). [99] A. R. Go~ni, K. Syassen, K. Str€ossner, and M. Cardona, Phys. Rev. B 39, 3178 (1989). [100] J. Chen, D. Patel, J. R. Sites, I. L. Spain, M. J. Hafich, and G. Y. Robinson, Solid State Commun. 75, 693 (1990). [101] J. Dong, G. Li, Z. Wang, D. Lu, X. Liu, X. Li, D. Sun, M. Kong, and Z. Wang, J. Appl. Phys. 79, 7177 (1996). [102] J. L. Aubel, U. K. Reddy, S. Sundaram, W. T. Beard, and J. Comas, J. Appl. Phys. 58, 495 (1985). [103] D. E. Aspnes, S. M. Kelso, R. A. Logan, and R. Bhat, J. Appl. Phys. 60, 754 (1986). [104] A. K. Saxena, Phys. Status Solidi B 105, 777 (1981). [105] B. Monemar, K. K. Shih, and G. D. Pettit, J. Appl. Phys. 47, 2604 (1976). [106] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [107] H. J. Lee, L. Y. Juravel, J. C. Woolley, and A. J. Spring Thorpe, Phys. Rev. B 21, 659 (1980). [108] J. C. M. Henning, J. P. M. Ansems, and P. J. Roksnoer, J. Phys. C: Solid State Phys. 19, L335 (1986). [109] B. Wakefield, M. A. G. Halliwell, T. Kerr, D. A. Andrews, G. J. Davies, and D. R. Wood, Appl. Phys. Lett. 44, 341 (1984). [110] W. Y. Chou, G. S. Chang, W. C. Hwang, and J. S. Hwang, J. Appl. Phys. 83, 3690 (1998). [111] D. Oertel, D. Bimberg, R. K. Bauer, and K. W. Carey, Appl. Phys. Lett. 55, 140 (1989). [112] A. Convertino, G. Padeletti, L. Cerri, and S. Viticoli, J. Vac. Sci. Technol. B 20, 243 (2002). [113] R. E. Nahory, M. A. Pollack, and J. C. DeWinter, J. Appl. Phys. 46, 775 (1975). [114] T. J. Kim, T. H. Ghong, Y. D. Kim, S. J. Kim, D. E. Aspnes, T. Mori, T. Yao, and B. H. Koo, Phys. Rev. B 68, 115323 (2003). [115] D. K. Gaskill, N. Bottka, L. Aina, and M. Mattingly, Appl. Phys. Lett. 56, 1269 (1990).

220

PROPERTIES OF SEMICONDUCTOR ALLOYS

[116] J. Singh, in Properties of Lattice-matched and Strained Indium Gallium Arsenide, EMIS Datareviews Series No. 8 (edited by P. Bhattacharya), INSPEC, London, 1993, p. 61. [117] L. C. Andreani, D. De Nova, S. Di Lernia, M. Geddo, G. Guizzetti, M. Patrini, C. Bocchi, A. Bosacchi, C. Ferrari, and S. Franchi, J. Appl. Phys. 78, 6745 (1995). [118] Z. Hang, D. Yan, F. H. Pollak, G. D. Pettit, and J. M. Woodall, Phys. Rev. B 44, 10546 (1991). [119] C. Alibert, A. Joullie, A. M. Joullie, and C. Ance, Phys. Rev. B 27, 4946 (1983), and references cited therein. [120] A. Bignazzi, E. Grilli, M. Guzzi, C. Bocchi, A. Bosacchi, S. Franchi, and R. Magnanini, Phys. Rev. B 57, 2295 (1998). [121] V. Bellani, M. Geddo, G. Guizzetti, S. Franchi, and R. Magnanini, Phys. Rev. B 59, 12272 (1999). [122] H. Mathieu, D. Auvergne, P. Merle, and K. C. Rustagi, Phys. Rev. B 12, 5846 (1975). [123] R. Ferrini, M. Patrini, and S. Franchi, J. Appl. Phys. 84, 4517 (1998). [124] S. G. Choi, C. J. Palmstrøm, Y. D. Kim, S. L. Cooper, and D. E. Aspnes, J. Appl. Phys. 98, 104108 (2005). [125] N. Kitamura, H. Yamamoto, and T. Wada, Mater. Lett. 15, 89 (1992). [126] S. Isomura, F. G. D. Prat, and J. C. Woolley, Phys. Status Solidi B 65, 213 (1974). [127] X. Yaozhou, Y. Beaulieu, and J. B. Webb, Solid State Commun. 87, 9 (1993). [128] N. Dai, F. Brown, R. E. Doezema, S. J. Chung, K. J. Goldammer, and M. B. Santos, Appl. Phys. Lett. 73, 3132 (1998). [129] S. M. Vishnubhatla, B. Eyglunent, and J. C. Woolley, Can. J. Phys. 47, 1661 (1969). [130] D. Auvergne, J. Camassel, H. Mathieu, and A. Joullie, J. Phys. Chem. Solids 35, 133 (1974). [131] A. P. Roth and E. Fortin, Can. J. Phys. 56, 1468 (1978). [132] R. Rousina, C. Halpin, and J. B. Webb, J. Appl. Phys. 68, 2181 (1990). [133] S. Collins, A. G. Birdwell, R. Glosser, and B. R. Bennett, J. Appl. Phys. 91, 1175 (2002). [134] S. Imai and S. Adachi, Jpn. J. Appl. Phys. 32, 3860 (1993). [135] See, for example, M. Henini, Dilute Nitride Semiconductors, Elsevier, Amsterdam, 2005. [136] U. Tisch, E. Finkman, and J. Salzman, Appl. Phys. Lett. 81, 463 (2002). [137] Y. Zhang, B. Fluegel, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 62, 4493 (2000). [138] Y. Zhang, B. Fluegel, M. C. Hanna, J. F. Geisz, L.-W. Wang, and A. Mascarenhas, Phys. Status Solidi B 240, 396 (2003). [139] W. Shan, W. Walukiewicz, J. W. Ager III, E. E. Haller, J. F. Geisz, D. J. Friedman, J. M. Olson, and S. R. Kurtz, Phys. Rev. Lett. 82, 1221 (1999). [140] W. Shan, W. Walukiewicz, K. M. Yu, J. Wu, J. W. Ager III, E. E. Haller, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 76, 3251 (2000). [141] P. R. C. Kent and A. Zunger, Phys. Rev. Lett. 86, 2613 (2001). [142] P. R. C. Kent and A. Zunger, Phys. Rev. B 64, 115208 (2001). [143] I. A. Buyanova, M. Izadifard, W. M. Chen, H. P. Xin, and C. W. Tu, Phys. Rev. B 69, 201303 (2004). [144] A. Mascarenhas, S. Francoeur, and S. Yoon, in Dilute Nitride Semiconductors (edited by M. Henini), Elsevier, Amsterdam, 2005, p. 179. [145] W. Walukiewicz, W. Shan, J. Wu, K. M. Yu, and J. W. Ager III, in Dilute Nitride Semiconductors (edited by M. Henini), Elsevier, Amsterdam, 2005, p. 325. [146] P. R. C. Kent, in Dilute Nitride Semiconductors (edited by M. Henini), Elsevier, Amsterdam, 2005, p. 393. [147] H. P. Xin, C. W. Tu, Y. Zhang, and A. Mascarenhas, Appl. Phys. Lett. 76, 1267 (2000). [148] I. A. Buyanova, G. Pozina, J. P. Bergman, W. M. Chen, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 81, 52 (2002). [149] G. Y. Rudko, I. A. Buyanova, W. M. Chen, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 81, 3984 (2002). [150] I. A. Buyanova, M. Izadifard, A. Kasic, H. Arwin, W. M. Chen, H. P. Xin, Y. G. Hong, and C. W. Tu, Phys. Rev. B 70, 085209 (2004). [151] D. G. Thomas, J. J. Hopfield, and C. J. Frosch, Phys. Rev. Lett. 15, 857 (1965).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

221

[152] G. Leibiger, V. Gottschalch, M. Schubert, G. Benndorf, and R. Schwabe, Phys. Rev. B 65, 245207 (2002). [153] J. Wu, W. Walukiewicz, K. M. Yu, J. W. Ager III, E. E. Haller, Y. G. Hong, H. P. Xin, and C. W. Tu, Phys. Rev. B 65, 241303 (2002). [154] L. Bellaiche, S.-H. Wei, and A. Zunger, Phys. Rev. B 56, 10233 (1997). [155] M. Weyers, M. Sato, and H. Ando, Jpn. J. Appl. Phys. 31, L853 (1992). [156] G. Pozina, I. Ivanov, B. Monemar, J. V. Thordson, and T. G. Andersson, J. Appl. Phys. 84, 3830 (1998). [157] R. Bhat, C. Caneau, L. Salamanca-Riba, W. Bi, and C. Tu, J. Cryst. Growth 195, 427 (1998). M. Schubert, G. Leibiger, V. Gottschalch, and G. Wagner, J. Appl. Phys. 89, 294 (2001). [158] J. Sik, [159] Y. Zhang, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 63, 161303 (2001). [160] J. Wu, W. Shan, and W. Walukiewicz, Semicond. Sci. Technol. 17, 860 (2002). [161] B. Gil, Solid State Commun. 114, 623 (2000). and M. Schubert, Appl. Phys. Lett. 77, 1650 [162] G. Leibiger, V. Gottschalch, B. Rheinl€ander, J. Sik, (2000). [163] J. Wagner, K. K€ohler, P. Ganser, and N. Herres, Appl. Phys. Lett. 77, 3592 (2000). [164] S. Matsumoto, H. Yaguchi, S. Kashiwase, T. Hashimoto, S. Yoshida, D. Aoki, and K. Onabe, J. Cryst. Growth 221, 481 (2000). and M. Schubert, J. Appl. Phys. 89, 4927 [165] G. Leibiger, V. Gottschalch, B. Rheinl€ander, J. Sik, (2001). [166] U. Tisch, E. Finkman, and J. Salzman, Phys. Rev. B 65, 153204 (2002). [167] A. Pulzara-Mora, E. Cruz-Hernandez, J. Rojas-Ramirez, R. Contreras-Cuerrero, M. MelendezLira, C. Falcony-Guajardo, M. A. Aguilar-Frutis, and M. L opez-L opez, J. Cryst. Growth 301–302, 565 (2007). [168] W. K. Hung, M. Y. Chern, Y. F. Chen, Z. L. Yang, and Y. S. Huang, Phys. Rev. B 62, 13028 (2000). [169] J. D. Perkins, A. Mascarenhas, Y. Zhang, J. F. Geisz, D. J. Friedman, J. M. Olson, and S. R. Kurtz, Phys. Rev. Lett. 82, 3312 (1999). [170] K. Uesugi, I. Suemune, T. Hasegawa, T. Akutagawa, and T. Nakamura, Appl. Phys. Lett. 76, 1285 (2000). [171] R. Chtourou, F. Bousbih, S. B. Bouzid, F. F. Charfi, J. C. Harmand, G. Ungaro, and L. Largeau, Appl. Phys. Lett. 80, 2075 (2002). [172] A. Polimeni, M. Bissiri, A. Augieri, G. B. H. von H€ ogersthal, M. Capizzi, D. Gollub, M. Fischer, M. Reinhardt, and A. Forchel, Phys. Rev. B 65, 235325 (2002). [173] J. Plaza, J. L. Casta~no, B. J. Garcia, H. Carrere, and E. Bedel-Pereira, Appl. Phys. Lett. 86, 121918 (2005). [174] B. S. Ma, F. H. Su, K. Ding, G. H. Li, Y. Zhang, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 71, 045213 (2005). [175] A. Kimura, C. A. Paulson, H. F. Tang, and T. F. Kuech, Appl. Phys. Lett. 84, 1489 (2004). [176] J. Wu, W. Walukiewicz, K. M. Yu, J. D. Denlinger, W. Shan, J. W. Ager III, A. Kimura, H. F. Tang, and T. F. Kuech, Phys. Rev. B 70, 115214 (2004). [177] W. G. Bi and C. W. Tu, Appl. Phys. Lett. 70, 1608 (1997). [178] P. H. Jefferson, T. D. Veal, L. F. J. Piper, B. R. Bennett, C. F. McConville, B. N. Murdin, L. Buckie, G. W. Smith, and T. Ashley, Appl. Phys. Lett. 89, 111921 (2006). [179] W. G. Bi and C. W. Yu, J. Appl. Phys. 80, 1934 (1996). [180] K. M. Yu, W. Walukiewicz, J. Wu, J. W. Beeman, J. W. Ager III, E. E. Haller, W. Shan, H. P. Xin, C. W. Tu, and M. C. Ridgway, J. Appl. Phys. 90, 2227 (2001). [181] H. Naoi, Y. Naoi, and S. Sakai, Solid-State Electron. 41, 319 (1997). [182] D.-K. Shih, H.-H. Lin, L.-W. Sung, T.-Y. Chu,and T.-R. Yang, Jpn. J. Appl. Phys. 42, 375 (2003). [183] M. Kuroda, R. Katayama, S. Nishio, K. Onabe, and Y. Shiraki, Phys. Status Solidi C 0, 2765 (2003). [184] T. D. Veal, L. F. J. Piper, P. H. Jefferson, I. Mahboob, C. F. McConville, M. Merrick, T. J. C. Hosea, B. N. Murdin, and M. Hopkinson, Appl. Phys. Lett. 87, 182114 (2005).

222

PROPERTIES OF SEMICONDUCTOR ALLOYS

[185] J. Wagner, K. K€ohler, P. Ganser, and M. Maier, Appl. Phys. Lett. 87, 051913 (2005). [186] B. N. Murdin, A. R. Adams, P. Murzyn, C. R. Pidgeon, I. V. Bradley, J.-P. R. Wells, Y. H. Matsuda, N. Miura, T. Burke, and A. D. Johnson, Appl. Phys. Lett. 81, 256 (2002). [187] T. D. Veal, I. Mahboob, and C. F. McConville, Phys. Rev. Lett. 92, 13801 (2004). [188] A.-B. Chen and A. Sher, Semiconductor Alloys: Physics and Materials Engineering, Plenum, New York, 1995. [189] F. Saadallah, N. Yacoubi, F. Genty, and C. Alibert, J. Appl. Phys. 94, 5041 (2003). [190] A. G. Thompson, M. Cardona, and K. L. Shaklee, Phys. Rev. 146, 601 (1966). [191] M. G. Craford, R. W. Shaw, A. H. Herzog, and W. O. Groves, J. Appl. Phys. 43, 4075 (1972). [192] A. G. Thompson, J. C. Woolley, and M. Rubenstein, Can. J. Phys. 44, 2927 (1966). [193] K. J. Kim, M. H. Lee, J. H. Bahng, K. Shim, and B. D. Choe, J. Appl. Phys. 84, 3696 (1998). [194] Z. I. Alferov, D. Z. Garbuzov, Y. V. Zhilyaev, and P. S. Kop’ev, Sov. Phys. Semicond. 6, 589 (1992). [195] H. Mathieu, P. Merle, and E. L. Ameziane, Phys. Rev. B 15, 2048 (1977). [196] M. J. Jou, Y. T. Cherng, H. R. Jen, and G. B. Stringfellow, J. Cryst. Growth 93, 62 (1988). [197] S. Loualiche, A. L. Corre, S. Salaun, J. Caulet, B. Lambert, M. Gauneau, D. Lecrosnier, and B. Deveaud, Appl. Phys. Lett. 59, 423 (1991). [198] R. E. Nahory, M. A. Pollack, J. C. DeWinter, and K. M. Williams, J. Appl. Phys. 48, 1607 (1977). [199] M. Yano, Y. Suzuki, T. Ishii, Y. Matsushita, and M. Kimata, Jpn. J. Appl. Phys. 17, 2091 (1978). [200] T. C. McGlinn, T. N. Krabach, and M. V. Klein, Phys. Rev. B 33, 8396 (1986). [201] R. Ferrini, M. Geddo, G. Guizzetti, M. Patrini, S. Franchi, C. Bocchi, F. Germini, A. Baraldi, and R. Magnanini, J. Appl. Phys. 86, 4706 (1999). [202] D. Serries, M. Peter, N. Herres, K. Winkler, and J. Wagner, J. Appl. Phys. 87, 8522 (2000). [203] K. G. Merkel, V. M. Bright, M. A. Marciniak, C. L. A. Cerny, and M. O. Manasreh, Appl. Phys. Lett. 65, 2442 (1994). [204] R. Lukic-Zrnic, B. P. Gorman, R. J. Cottier, T. D. Golding, C. L. Littler, and A. G. Norman, J. Appl. Phys. 92, 6939 (2002). [205] H. Chouaib, C. Bru-Chevallier, G. Guillot, H. Lahreche, and P. Bove, J. Appl. Phys. 98, 123524 (2005). [206] G. A. Antypas and T. O. Yep, J. Appl. Phys. 42, 3201 (1971). [207] R. J. Nicholas, R. A. Stradling, and J. C. Ramage, J. Phys. C: Solid State Phys. 12, 1641 (1979). [208] M. Wada, S. Araki, T. Kudou, T. Umezawa, S. Nakajima, and T. Ueda, Appl. Phys. Lett. 76, 2722 (2000). [209] S. S. Bui, H. P. Lee, and K. M. Yu, Appl. Phys. Lett. 90, 212113 (2007). [210] A. G. Thompson, J. E. Rowe, and M. Rubenstein, Phys. Rev. 40, 3280 (1969). [211] S. G. Choi, C. J. Palmstrøm, Y. D. Kim, D. E. Aspnes, H. J. Kim, and Y.-C. Chang, Appl. Phys. Lett. 91, 041917 (2007). [212] E. H. Reihlen, M. J. Jou, Z. M. Fang, and G. B. Stringfellow, J. Appl. Phys. 68, 4604 (1990). [213] W. J. Duncan, A. S. M. Ali, E. M. Marsh, and P. C. Spurdens, J. Cryst. Growth 143, 155 (1994). [214] J. C. Woolley and J. Warner, Can. J. Phys. 42, 1879 (1964). [215] G. B. Stringfellow and P. E. Greene, J. Electrochem. Soc. 118, 805 (1971). [216] W. Dobbelaere, J. D. Boeck, and G. Borghs, Appl. Phys. Lett. 55, 1856 (1989). [217] H. Y. Deng and N. Dai, Phys. Rev. B 73, 113102 (2006). [218] S. Elies, A. Krier, I. R. Cleverley, and K. Singer, J. Phys. D: Appl. Phys. 26, 159 (1993). [219] M. A. Marciniak, R. L. Hengehold, Y. K. Yeo, and G. W. Turner, J. Appl. Phys. 84, 480 (1998). [220] B. Bansal, V. K. Dixit, V. Venkataraman, and H. L. Bhat, Appl. Phys. Lett. 82, 4720 (2003). [221] V. K. Dixit, B. Bansal, V. Venkataraman, H. L. Bhat, K. S. Chandrasekharan, and B. M. Arora, J. Appl. Phys. 96, 4989 (2004). [222] Y. Z. Gao, X. Y. Gong, Y. H. Chen, and T. Yamaguchi, Proc. SPIE 6029, 60291I (2006). [223] Y. G. Hong, A. Nishikawa, and C. W. Tu, Appl. Phys. Lett. 83, 5446 (2003). [224] I. A. Buyanova, M. Izadifard, W. M. Chen, Y. G. Hong, and C. W. Tu, Appl. Phys. Lett. 88, 031907 (2006).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

223

[225] K. I. Lin, T. S. Wang, Y. T. Lu, and J. S. Hwang, J. Appl. Phys. 99, 056103 (2006). [226] K. I. Lin and J. S. Hwang, Appl. Phys. Lett. 89, 192116 (2006). [227] A. E. Zhukov. A. R. Kovsh, E. S. Semenova, V. M. Ustinov, L. Wei J.-S. Wang, and J. Y. Chi, Semicond. 36, 899 (2002). [228] Z. Pan, L. H. Li, Y. W. Lin, B. Q. Sun, D. S. Jiang, and W. K. Ge, Appl. Phys. Lett. 78, 2217 (2001). [229] S. A. Choulis, T. J. C. Hosea, S. Tomic, M. Kamal-Saadi, A. R. Adams, E. P. O’Reilly, B. A. Weinstein, and P. J. Klar, Phys. Rev. B 66, 165321 (2002). [230] A. Polimeni, M. Capizzi, M. Geddo, M. Fischer, M. Reinhardt, and A. Forchel, Phys. Rev. B 63, 195320 (2001). [231] H. D. Sun, M. D. Dawson, M. Othman, J. C. L. Yong, J. M. Rorison, P. Gilet, L. Grenouillet, and A. Million, Appl. Phys. Lett. 82, 376 (2003). [232] D. Serries, T. Geppert, P. Ganser, M. Maier, K. K€ohler, N. Herres, and J. Wagner, Appl. Phys. Lett. 80, 2448 (2002). [233] C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002), and references cited therein. [234] P. Perlin, S. G. Subramanya, and D. E. Mars, Appl. Phys. Lett. 73, 3703 (1998). [235] C. Skierbiszewski, P. Erlin, P. Wisniewski, T. Suski, J. F. Geisz, K. Hingerl, W. Jantsch, D. E. Mars, and W. Walukiewicz, Phys. Rev. B 65, 035207 (2001). [236] M. M. E. Fahmi, A. Khan, J. A. Griffin, G. L. Harris, L. H. Robins, A. G. Birdwell, Y.-S. Kang, D. J. Smith, T. Steiner, and S. N. Mohammad, J. Appl. Phys. 94, 7576 (2003). [237] Y.-S. Kang, L. H. Robins, A. G. Birdwell, A. J. Shapiro, W. R. Thurber, M. D. Vaudin, M. M. E. Fahmi, D. Bryson, and S. N. Mohammad, J. Appl. Phys. 98, 093714 (2005). [238] L. Bellaiche, Appl. Phys. Lett. 75, 2578 (1999). [239] K. M. Yu, W. Walukiewicz, J. W. Ager III, D. Bour, R. Farshchi, O. D. Dubon, S. X. Li, I. D. Sharp, and E. E. Haller, Appl. Phys. Lett. 88, 092110 (200). [240] J. H. Herrera-Perez, M. B. Z. Morosini, and N. P. Patel, in Proceedings of the 5th Brazilian School on Semiconductor Physics (edited by J. R. Leite, A. Fazzio, and A. S. Chaves), World Scientific, Singapore, 1991, p. 395. [241] N. Yacoubi, A. Hafaiedh, and A. Joullie, Appl. Opt. 33, 7171 (1994). [242] D. O. T. Filho, I. F. L. Dias, E. Laureto, J. L. Duarte, S. A. Louren˛c o, L. C. Po˛c as, S. S. Prabhu, and J. Klem, J. Appl. Phys. 97, 123702 (2005). [243] S. P. Svensson, D. M. Gill, and P. N. Uppal, J. Appl. Phys. 81, 1422 (1997). [244] N. A. Charykov, A. M. Litvak, K. D. Moiseev, and Y. P. Yakovlev, Proc. SPIE 1512, 198 (1991). [245] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992. [246] S. Shirakata, M. Kondo, T. Nishino, and Y. Hamakawa, Jpn. J. Appl. Phys. 25, 435 (1986). [247] G. P. Donati, R. Kaspi, and K. J. Malloy, J. Appl. Phys. 94, 5814 (2003). [248] L. I. Kamlet and F. L. Terry, Jr., J. Electron. Mater. 24, 2005 (1995). [249] C. Reh and G. Weiser, Phys. Rev. B 65, 035321 (2001). [250] J. C. DeWinter, M. A. Pollack, A. K. Srivastava, and J. L. Zyskind, J. Electron. Mater. 14, 729 (1985). [251] T. I. Voronina, T. S. Lagunova, M. P. Mikhailova, M. A. Sipovskaya, V. V. Sherstnev, and Y. P. Yakoviev, Sov. Phys. Semicond. 25, 167 (1991). [252] M. P. Mikhailova and A. N. Titkov, Semicond. Sci. Technol. 9, 1279 (1994). [253] M. J. Cherng, G. B. Stringfellow, D. W. Kisker, A. K. Srivastava, and J. L. Zyskind, Appl. Phys. Lett. 48, 419 (1986). [254] T. Mei, J. Appl. Phys. 101, 013520 (2007). [255] S. Iyer, S. Hegde, K. K. Bajaj, A. Abul-Fadl, and W. Mitchel, J. Appl. Phys. 73, 3958 (1993). [256] M. Mu~noz, F. H. Pollak, M. B. Zakia, N. B. Patel, and J. L. Herrera-Perez, Phys. Rev. B 62, 16600 (2000). [257] X. Gong, H. Kan, T. Yamaguchi, I. Suzuki, M. Aoyama, M. Kumagawa, N. L. Rowell, A. Wang, and R. Rinfret, Jpn. J. Appl. Phys. 33, 1740 (1994).

224

PROPERTIES OF SEMICONDUCTOR ALLOYS

[258] D. J. Mowbray, O. P. Kowalski, M. Hopkinson, and J. P. R. David, Appl. Phys. Lett. 65, 213 (1994). [259] S. P. Najda, A. H. Kean, M. D. Dawson, and G. Duggan, J. Appl. Phys. 77, 3412 (1995). [260] M. Schubert, J. A. Woollam, G. Leibiger, B. Rheinl€ander, I. Pietzonka, T. Sab, and V. Gottschalch, J. Appl. Phys. 86, 2025 (1999). [261] K. Asami, H. Asahi, S. Gonda, Y. Kawamura, and H. Tanaka, Solid State Commun. 70, 33 (1989). [262] D. S. Cao, A. W. Kimball, and G. B. Stringfellow, J. Appl. Phys. 67, 739 (1990). [263] S. Adachi, S. Ozaki, M. Sato, and K. Ohtsuka, Jpn. J. Appl. Phys. 35, 537 (1996). [264] S. Ozaki, S. Adachi, M. Sato, and K. Ohtsuka, J. Appl. Phys. 79, 439 (1996). [265] H. Lee, M. V. Klein, D. E. Aspnes, C. P. Kuo, M. Peanasky, and M. G. Craford, J. Appl. Phys. 73, 400 (1993). [266] A. D. Prins, J. L. Sly, A. T. Meney, D. J. Dunstan, E. P. O’Reilly, A. R. Adams, and A. Valster, J. Phys. Chem. Solids 56, 349 (1995). [267] J. Harada, T. Kobayashi, A. D. Prins, and D. J. Dunstan, Phys. Status Solidi B 235, 505 (2003). [268] J. I. Davies, A. C. Marshall, M. D. Scott, and R. J. M. Griffiths, Appl. Phys. Lett. 53, 276 (1988). [269] C. Cacciatore, D. Campi, C. Coriasso, C. Rigo, and C. Alibert, Thin Solid Films 197, 1 (1991). [270] W. F. Tseng, J. Comas, B. Steiner, G. Metze, A. Cornfeld, P. B. Klein, D. K. Gaskill, W. Xia, and S. S. Lau, Mater. Res. Soc. Symp. Proc. 240, 117 (1992). [271] R. F. Kopf, H. P. Wei, A. P. Perley, and G. Livescu, Appl. Phys. Lett. 60, 2386 (1992). [272] P. Parayanthal, C. S. Ro, F. H. Pollak, C. R. Stanley, G. W. Wicks, and L. F. Eastman, Appl. Phys. Lett. 43, 109 (1983). [273] J.-W. Pan, J.-L. Shieh, J.-H. Gau, J.-I. Chyi, J.-C. Lee, and K.-J. Ling, J. Appl. Phys. 78, 442 (1995). [274] S. N. Grinyaev, L. M. Dolginov, M. A. Il’in, Y. N. Korchagin, A. I. Lukomskiı, and V. A. Chaldyshev, Sov. Phys. Semicond. 16, 467 (1982). [275] H. Mani, E. Tournie, J. L. Lazzari, C. Alibert, A. Joullie, and B. Lambert, J. Cryst. Growth 121, 463 (1992). [276] L.-C. Chen, W.-J. Ho, and M.-C. Wu, Jpn. J. Appl. Phys. 38, 1314 (1999). [277] Y. R. Ryu, T. S. Lee, J. A. Lubguban, A. B. Corman, H. W. White, J. H. Leem, M. S. Han, Y. S. Park, C. J. Youn, and W. J. Kim, Appl. Phys. Lett. 88, 052103 (2006). [278] M. S. Han, J. H. Kim, T. S. Jeong, J. M. Park, C. J. Youn, J. H. Leem, and Y. R. Ryu, J. Cryst. Growth 303, 506 (2007). [279] T. Makino, Y. Segawa, M. Kawasaki, A. Ohtomo, R. Shiroki, K. Tamura, T. Yasuda, and H. Koinuma, Appl. Phys. Lett. 78, 1237 (2001). [280] R. Schmidt-Grund, M. Schubert, B. Rheinl€ander, D. Fritsch, H. Schmidt, E. M. Kaidashev, M. Lorenz, C. M. Herzinger, and M. Grundmann, Thin Solid Films 455–456, 500 (2004). [281] K. Koike, K. Hama, I. Nakashima, G. Takada, K. Ogata, S. Sasa, M. Inoue, and M. Yano, J. Cryst. Growth 278, 288 (2005). [282] R. Schmidt-grund, A. Carstens, B. Rheinl€ander, D. Spemenn, H. Hochmut, G. Zimmermann, M. Lorenz, and M. Grundmann, J. Appl. Phys. 99, 123701 (2006). [283] N. B. Chen and C. H. Sui, Mater. Sci. Eng. B 126, 16 (2006). [284] J. A. Sans and A. Segura, High Pressure Res. 24, 119 (2004). [285] J. Ishihara, A. Nakamura, S. Shigemori, T. Aoki, and J. Temmyo, Appl. Surf. Sci. 244, 381 (2005), and references cited therein. [286] X. J. Wang, I. A. Buyanova, W. M. Chen, M. Izadifard, S. Rawal, D. P. Norton, S. J. Pearton, A. Osinsky, J. W. Dong, and A. Dabiran, Appl. Phys. Lett. 89, 151909 (2006). [287] H. S. Kang, J. W. Kim, J. H. Kim, S. Y. Lee, Y. Li, J.-S. Lee, J. K. Lee, M. A. Nastasi, S. A. Crooker, and Q. X. Jia, J. Appl. Phys. 99, 066113 (2006). [288] H. C. Ong and J. Y. Dai, Appl. Phys. Lett. 81, 1444 (2002). [289] K. Ichino, K. Ueyama, M. Yamamoto, H. Kariya, H. Miyata, H. Misasa, M. Kitagawa, and H. Kobayashi, J. Appl. Phys. 87, 4249 (2000). [290] G. K. Padam, G. L. Malhotra, and S. U. M. Rao, J. Appl. Phys. 63, 770 (1988). [291] A. Beliveau and C. Carlone, Phys. Rev. B 41, 9860 (1990).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS [292] [293] [294] [295] [296] [297] [298] [299] [300] [301] [302] [303] [304] [305] [306] [307] [308] [309] [310] [311] [312] [313] [314] [315] [316] [317] [318] [319] [320] [321] [322] [323] [324]

225

V. Kumar, V. Singh, S. K. Sharma, and T. P. Sharma, Opt. Mater. 11, 29 (1998). A. M. Salem, Appl. Phys. A 74, 205 (2002). T. Yokogawa, T. Ishikawa, J. L. Merz, and T. Taguchi, J. Appl. Phys. 75, 2189 (1994). M. R. Muhamad, Jpn. J. Appl. Phys. 32, 3385 (1993). A. Kremheller, A. K. Levine, and G. Gashurov, J. Electrochem. Soc. 107, 12 (1960). E. S. Rittner and J. H. Schulman, J. Phys. Chem. 47, 537 (1943). K. Wilmers, T. Wethkamp, N. Esser, C. Cobet, W. Richter, V. Wagner, H. Lugauer, F. Fischer, T. Gerhard, M. Keim, and M. Cardona, J. Electron. Mater. 28, 670 (1999). A. Bukaluk, A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Ł e˛ gowski, H. M e˛ czynska, and J. Szatkowski, Appl. Surf. Sci. 175–176, 531 (2001). G. P. Srivastava, H. M. T€ut€unc€u, and N. G€unhan, Phys. Rev. B 70, 085206 (2004). C. Chauvet, E. Tournie, and J.-P. Faurie, Phys. Rev. B 61, 5332 (2000). C. Chauvet, E. Tournie, and J.-P. Faurie, J. Cryst. Growth 214/215, 95 (2000). H. Lee, I.-Y. Kim, J. Powell, D. E. Aspnes, S. Lee, F. Peiris, and J. K. Furdyna, J. Appl. Phys. 88, 878 (2000). S. V. Ivanov, O. V. Nekrutkina, S. V. Sorokin, V. A. Kaygorodov, T. V. Shubina, A. A. Toropov, P. S. Kop’ev, G. Reuscher, V. Wagner, J. Geurts, A. Waag, and G. Landwehr, Appl. Phys. Lett. 78, 404 (2001). O. Maksimov, M. Mu~noz, and M. C. Tamargo, Microelectron. J. 37, 19 (2006). P. J. Huang, P. Sitarek, Y. S. Huang, O. Maksimov, M. C. Tamargo, F. Firszt, and H. M e˛ czy nska, Phys. Status Solidi C 3, 738 (2006). A. A. Wronkowska, A. Wronkowski, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, A. Marasek, and W. Paszkowicz, Phys. Status Solidi C 1, 641 (2004). F. Firszt, S. Ł e˛ gowski, H. M e˛ czynska, H. L. Oczkowski, W. Osi nska, J. Szatkowski, W. Paszkowicz, and Z. M. Spolnik, J. Cryst. Growth 159, 167 (1996). B. Jobst, D. Hommel, U. Lunz, T. Gerhard, and G. Landwehr, Appl. Phys. Lett. 69, 97 (1996). H. Okuyama, Y.Kishita, and A. Ishibashi, Phys. Rev. B 57, 2257 (1998). K. J. Kim, M. H. Lee, J. H. Bahng, C. Y. Kwak, and E. Oh, Solid State Commun. 105, 17 (1998). M. Sohel, M. Mu~noz, and M. C. Tamargo, Appl. Phys. Lett. 85, 2794 (2004). R. P€assler, F. Blaschta, E. Griebl, K. Papagelis, B. Haserer, T. Reisinger, S. Ves, and W. Gebhardt, Phys. Status Solidi B 204, 685 (1997). A. Gapinski and W. Bała, Proc. SPIE 3725, 72 (1999). W.-T. Kim, Phys. Rev. B 59, 4572 (1999). A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, and J. Szatkowski, Vacuum 63, 233 (2001). F. Firszt, A. A. Wronkowska, A. Wronkowski, S. Ł e˛ gowski, A. Marasek, H. M e˛ czy nska, M. Pawlak, W. Paszkowicz, K. Strzałkowski, and A. J. Zakrzewski, Cryst. Res. Technol. 40, 386 (2005). D.-T. Kim, S.-A. Park, W.-J. Jeong, C.-C. Park, M.-S. Jin, and C.-D. Kim, Phys. Status Solidi C 3, 2665 (2006). V. A. Kaygorodov, I. V. Sedova, S. V. Sorokin, A. A. Sitnikova, O. V. Nekrutkina, T. V. Shubina, A. A. Toropov, V. S. Sorokin, and S. V. Ivanov, Phys. Status Solidi B 229, 19 (2002). C.-D. Kim, D.-H. Shin, H.-H. Jang, H.-M. Jeong, D.-T. Kim, C.-S. Yoon, H.-L. Park, and W.-T. Kim, J. Appl. Phys. 85, 7972 (1999). P. J. Huang. Y. S. Huang, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, and K. K. Tiong, J. Phys.: Condens. Matter 19, 266002 (2007). A. S. Nasibov, Y. V. Korostelin, P. V. Shapkin, L. G. Suslina, D. L. Fedorov, and L. S. Markov, Solid State Commun. 71, 867 (1989). N. Samarth, H. Luo, J. K. Furdyna, R. G. Alonso, Y. R. Lee, A. K. Ramdas, S. B. Qadri, and N. Otsuka, Appl. Phys. Lett. 56, 1163 (1990). Y. D. Kim, M. V. Klein, S. F. Ren, Y. C. Chang, H. Luo, N. Samarth, and J. K. Furdyna, Phys. Rev. B 49, 7262 (1994).

226

PROPERTIES OF SEMICONDUCTOR ALLOYS

[325] U. Lunz, J. Kuhn, F. Goschenhofer, U. Sch€ussler, S. Einfeldt, C. R. Becker, and G. Landwehr, J. Appl. Phys. 80, 6861 (1996). [326] J. Lee, F. Flack, N. Samarth, and R. W. Collins, Appl. Opt. 36, 5372 (1997). [327] L. Malikova, W. Krystek, F. H. Pollak, N. Dai, A. Cavus, and M. C. Tamargo, Phys. Rev. B 54, 1819 (1996). [328] M.-C. Kuo, K.-C. Chiu, T.-H. Shin, Y.-J. Lai, C.-S. Yang, W.-K. Chen, D.-S. Chuu, M.-C. Lee, W.-C. Chou, S.-Y. Jeng, Y.-T. Shin, and W.-H. Lan, Jpn. J. Appl. Phys. 43, 5145 (2004). [329] A. Kalb and V. Leute, Phys. Status Solidi A 5, K199 (1971). [330] C. J. Summers and J. G. Broerman, Phys. Rev. B 21, 559 (1980). [331] N. Himei and J. Muto, J. Mater. Sci.: Mater. Electron. 11, 145 (2000). [332] V. B. Pujari, S. H. Mane, V. S. Karande, J. S. Dargad, and L. P. Deshmukh, Mater. Chem. Phys. 83, 10 (2004). [333] I. N. Borisov, P. S. Kireev, V. V. Mikhailin, and V. M. Bezborodova, Sov. Phys. Semicond. 5, 734 (1971). [334] K. Kumazaki, L. Vi~na, C. Umbach, and M. Cardona, Phys. Status Solidi B 156, 371 (1989). [335] O. Maksimov and M. C. Tamargo, Appl. Phys. Lett. 79, 782 (2001). [336] M. R. Buckley, F. C. Peiris, O. Maksimov, M. Mu~ noz, and M. C. Tamargo, Appl. Phys. Lett. 81, 5156 (2002). [337] M. Mu~noz, O. Maksimov, M. C. Tamargo, M. R. Buckley, and F. C. Peiris, Phys. Status Solidi C 1, 706 (2004). [338] J. Zakrzewski, Proc. SPIE 5953, 595307 (2005). [339] S. G. Parker, A. R. Reinberg, J. E. Pinnell, and W. C. Holton, J. Electrochem. Soc. 118, 979 (1971). [340] D. Barbier, B. Montegu, and A. Laugier, Solid State Commun. 28, 525 (1978). [341] S.-J. Chung, Y. Kwon, C.-S. Yoon, B.-H. Kim, D. Cha, C.-D. Kim, W.-T. Kim, and C. U. Hong, J. Phys. Chem. Solids 60, 799 (1999). [342] A. J. Franz, F. C. Peiris, X. Liu, U. Bindley, and J. K. Furdyna, Phys. Status Solidi B 241, 507 (2004). [343] K. Itoh, J. Phys. Soc. Jpn 22, 1119 (1967). [344] M. Luttmann, F. Bertin, and A. Chabli, J. Appl. Phys. 78, 3387 (1995). [345] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, I. Miotkowski, and A. K. Ramdas, Appl. Phys. Lett. 71, 249 (1997). [346] Y. S. Ihn, T. J. Kim, T. H. Ghong, Y. D. Kim, D. E. Aspnes, and J. Kossut, Thin Solid Films 455–456, 222 (2004). [347] B. Freytag, J. Phys.: Condens. Matter 6, 9875 (1994). [348] K. Saito, A. Ebina, and T. Takahashi, Solid State Commun. 11, 841 (1972). [349] V. A. Tyagai, O. V. Snitko, V. N. Bondarenko, N. I. Vitrikhovskii, V. B. Popov, and A. N. Krasiko, Sov. Phys. Solid State 16, 885 (1974). [350] V. V. Sobolev, O. G. Maksimova, and S. G. Kroitoru, Phys. Status Solidi B 499 (1981). [351] S. Adachi and T. Kimura, Jpn. J. Appl. Phys. 32, 3496 (1993). [352] O. Castaing, R. Granger, J. T. Benhlal, and R. Triboulet, J. Phys.: Condens. Matter 8, 5757 (1996). [353] K. P. Rao, O. M. Hussain, K. T. R. Reddy, P. S. Reddy, S. Uthanna, B. S. Naidu, and P. J. Reddy, Opt. Mater. 5, 63 (1996). [354] P. D. Paulson, B. E. McCandless, and R. W. Birkmire, J. Appl. Phys. 95, 3010 (2004). [355] A. Kisiel, Acta Phys. Polon. A 38, 691 (1970). [356] E. M. Larramendi, E. Puron, and O. de Melo, Semicond. Sci. Technol. 17, 8 (2002). [357] F. G. Sanchez-Almazan, H. Navarro-Contreras, G. Ramırez-Flores, M. A. Vidal, O. Zelaya-Angel, M. E. Rodrıguez, and R. Baquero, J. Appl. Phys. 79, 7713 (1996). [358] O. Zelaya-Angel, J. G. Mendoza-Alvarez, M. Becerril, H. Navarro-Contreras, and L. TiradoMejia, J. Appl. Phys. 95, 6284 (2004). [359] Y. T. Shih, W. C. Fan, C. S. Yang, M. C. Kuo, and W. C. Chou, J. Appl. Phys. 94, 3791 (203). [360] B. Toulouse, R. Granger, S. Rolland, and R. Triboulet, J. Phys. 48, 247 (1987).

ENERGY-BAND STRUCTURE: ENERGY-BAND GAPS

227

[361] D. Lemoine, K. H. Khelladi, O. Castaing, J. Benhlal, A. Quemerais, I. Pollini, R. Triboulet, and R. Granger, Mater. Sci. Eng. B 28, 39 (1994). [362] F. El-Akkad and A. R. Farhan, J. Phys. D: Appl. Phys. 28, 1958 (1995). [363] O. Casting, J. T. Benhlal, R. Granger, and R. Triboulet, J. Phys. I France 6, 907 (1996). [364] V. G. Sredin, V. G. Savitskiı, Y. V. Danilyuk, M. V. Miliyanchuk, and I. V. Petrovich, Sov. Phys. Semicond. 15, 249 (1981). [365] J. P. Laurenti, J. Camassel, A. Bouhemadou, B. Toulouse, R. Legros, and A. Lusson, J. Appl. Phys. 67, 6454 (1990). [366] J. Chu, Z. Mi, and D. Tang, Infrared Phys. 32, 195 (1991). [367] A. Rodzik and A. Kisiel, J. Phys. C: Solid State Phys. 16, 203 (1983). [368] A. Moritani, K. Taniguchi, C. Hamaguchi, J. Nakai, R. Ueda, and O. Ohtsuki, J. Phys. Soc. Jpn. 31, 945 (1971). [369] L. Vi~na, C. Umbach, M. Cardona, and L. Vodopyanov, Phys. Rev. B 29, 6752 (1984). [370] H. Arwin and D. E. Aspnes, J. Vac. Sci. Technol. A 2, 1316 (1984). [371] M. W. Scott, J. Appl. Phys. 40, 4077 (1969). [372] G. L. Hansen, J. L. Schmit, and T. N. Casselman, J. Appl. Phys. 53, 7099 (1982). [373] A. Ksendzov, F. H. Pollak, J. A. Wilson, and V. A. Cotton, J. Appl. Phys. 66, 5528 (1989). [374] C. C. Kim and S. Sivananthan, J. Electron. Mater. 26, 561 (1997). [375] C.-Y. Moon, S.-H. Wei, Y. Z. Zhu, and G. D. Chen, Phys. Rev. B 74, 233202 (2006). [376] B. K. Meyer, A. Polity, B. Farangis, Y. He, D. Hasselkamp, T. Kr€amer, and C. Wang, Appl. Phys. Lett. 85, 4929 (2004). [377] Y. Nabetani, T. Mukawa, Y. Ito, T. Kato, and T. Matsumoto, Appl. Phys. Lett. 83, 1148 (2003). [378] W. Shan, W. Walukiewicz, J. W. Ager III, K. M. Yu, J. Wu, E. E. Haller, Y. Nabetani, T. Murakawa, Y. Ito, and T. Matsumoto, Appl. Phys. Lett. 83, 299 (2003). [379] A. Polimeni, M. Capizzi, Y. Nabetani, Y. Ito, K. Kato, T. Matsumoto, and T. Hirai, Appl. Phys. Lett. 84, 3304 (2004). [380] A. Ebina, E. Fukunaga, and T. Takahashi, Phys. Rev. B 10, 2495 (1974). [381] H. Araki, H. Kanie, and M. Sano, Jpn. J. Appl. Phys. 33, 235 (1994). [382] E. Griebl, G. F. Sch€otz, C. Birzer, W. Kerner, T. Reisinger, B. Hahn, and W. Gebhardt, Acta Phys. Polon. A 88, 995 (1995). [383] P. R. Newbury, K. Shahzad, J. Petruzzello, and D. A. Cammack, J. Appl. Phys. 66, 4950 (1989). [384] R. Hill and D. Richardson, J. Phys. C: Solid State Phys. 6, L115 (1973). [385] Y.-M. Yu, S. Nam, J.-K. Rhee, B. O, K.-S. Lee, and Y. D. Choi, J. Cryst. Growth 210, 521 (2000). [386] W. Walukiewicz, W. Shan, K. M. Yu, J.W. Ager III, E. E. Haller, I. Miotkowski, M. J. Seong, H. Alawadhi, and A. K. Ramdas, Phys. Rev. Lett. 85, 1552 (2000). [387] C. Y. Bang, M. S. Lee, T. J. Kim, Y. D. Kim, D. E. Aspnes, Y. M. Yu, B. O, and Y. D. Choi, J. Kor. Phys. Soc. 39, 462 (2001). [388] S. Larach, R. E. Shrader, and C. F. Stocker, Phys. Rev. 108, 587 (1957). [389] A. Ebina, M. Yamamoto, and T. Takahashi, Phys. Rev. B 6, 3786 (1972). [390] M. J. S. P. Brasil, R. E. Nahory, F. S. Turco-Sandroff, H. L. Gilchrist, and R. J. Martin, Appl. Phys. Lett. 58, 2509 (1991). [391] C.-H. Su, S. Feth, S. Zhu, S. L. Lehoczky, and L. J. Wang, J. Appl. Phys. 88, 5148 (2000). [392] H. Lee, S. M. Kim, B. Y. Seo, E. Z. Seong, S. H. Choi, S. Lee, and J. K. Furdyna, Appl. Phys. Lett. 77, 2997 (2000). [393] A. Naumov, H. Stanzl, K. Wolf, S. Lankes, and W. Gebhardt, J. Appl. Phys. 74, 6178 (1993). [394] J. Wu, W. Walukiewicz, K. M. Yu, W. Shan, J. W. Ager III, E. E. Haller, I. Miotkowski, A. K. Ramdas, and C.-H. Su, Phys. Rev. B 68, 033206 (2003). [395] V. N. Bondarenko, N. I. Vitrikhovskii, and V. A. Tyagai, Sov. Phys. Solid State 13, 1854 (1972). [396] G. Perna, S. Pagliara, V. Capozzi, M. Ambrico, and M. Pallara, Solid State Commun. 114, 161 (2000). [397] R. L. Hengehold and C. R. Fraime, Phys. Rev. 174, 808 (1968).

228 [398] [399] [400] [401] [402] [403] [404] [405] [406] [407] [408] [409] [410] [411] [412] [413] [414] [415] [416] [417]

PROPERTIES OF SEMICONDUCTOR ALLOYS D. W. Lane, Sol. Ener. Mater. Sol. Cells 90, 1169 (2006). K. Ohata, J. Saraie, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1641 (1973). K. Wei, F. H. Pollak, J. L. Freeouf, D. Shvydka, and A. D. Compaan, J. Appl. Phys. 85, 7418 (1999). P. J. Sebastian and V. Sivaramakrishnan, J. Cryst. Growth 112, 421 (1991). M. Schenk and C. Silber, J. Mater. Sci.: Mater. Electron. 9, 295 (1998). Z. C. Feng, P. Becla, L. S. Kim, S. Perkowitz, Y. P. Feng, H. C. Poon, K. P. Williams, and G. D. Pitt, J. Cryst. Growth 138, 239 (1994). G. Brill, Y. Chen, P. M. Amirtharaj, W. Sarney, D. Chandler-Horowitz, and N. K. Dhar, J. Electron. Mater. 34, 655 (2005). J. M. Gaines, R. R. Drenten, K. W. Haberern, T. Marshall, P. Mensz, and J. Petruzzello, Appl. Phys. Lett. 62, 2462 (1993). U. Lunz, B. Jobst, S. Einfeldt, C. R. Becker, D. Hommel, and G. Landwehr, J. Appl. Phys. 77, 5377 (1995). H. J. Chen, D. Y. Lin, Y. S. Huang, R. C. Tu, Y. K. Su, and K. K. Tiong, Semicond. Sci. Technol. 14, 85 (1999). K. Naniwae, H. Iwata, and K. Yashiki, Appl. Phys. Lett. 74, 3984 (1999). K. Shim, H. Rabitz, J.-H. Chang, and T. Yao, J. Cryst. Growth 214/215, 350 (2000). V. Wagner, A. Fleszar, J. Geurts, G. Reusher, M. Keim, A. Waag, G. Landwehr, K. Wilmers, N. Esser, and W. Richter, J. Cryst. Growth 214/215, 340 (2000). K. Godo, H. Makino, M. W. Cho, J. H. Chang, Y. Yamazaki, T. Yao, M. Y. Shen, and T. Goto, Appl. Phys. Lett. 79, 4168 (2001). P. J. Huang, H. P. Hsu, Y. S. Huang, F. Firzt, S. L e˛ gowski, H. M e˛ czy nska, A. Marasek, and K. K. Tiong, J. Appl. Phys. 102, 083515 (2007). Y. T. Liu, P. Sitarek, Y. S. Huang, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, A. Marasek, W. Paszkowicz, and K. K. Tiong, J. Appl. Phys. 98, 083519 (2005). A. A. Wronkowska, F. Firszt, H. Arwin, A. Wronkowski, M. Wakula, K. Strzalkowski, and W. Paszkowicz, Phys. Status Solidi C 3, 1193 (2006). J. W. Wang, P. J. Huang, H. P. Hsu, Y. S. Huang, F. Firszt, S. Ł e˛ gowski, H. M e˛ czy nska, A. Marasek, and K. K. Tiong, J. Appl. Phys. 101, 103539 (2007). C.-H. Hsieh, Y.-S. Huang, C.-H. Ho, K.-K. Tiong, M. Mu~ noz, O. Maksimov, and M. C. Tamargo, Jpn. J. Appl. Phys. 43, 459 (2004). O. Maksimov, M. Mu~noz, W. H. Wang, M. C. Tamargo, and N. Samarth, Phys. Status Solidi B 241, R5 (2004).

7 Energy-band Structure: Effective Masses 7.1 INTRODUCTORY REMARKS 7.1.1 Electron Effective Mass The constant-energy surface in semiconductors can be defined by E¼

h2 k2y h2 k2z 2 k2x h þ þ 2mx 2my 2mz

ð7:1Þ

where the electron at the center of the BZ has a spherical constant-energy surface (i.e. mx ¼ my ¼ mz), while there are six constant-energy ellipsoids along the principal diagonal [100] and its equivalent directions and eight ellipsoids along the h111i directions [1]. In such ellipsoidal constant-energy surfaces, Equation (7.1) can be simply written as E¼

2 k2t h h2 k2l þ mt 2ml

ð7:2Þ

The two masses ml and mt in Equation (7.2) are the longitudinal mass and transverse mass, respectively, because ml (mz) is defined along the h100i axis (X valley) and along the h111i axis (L valley), whereas mt (mx ¼ my) is defined in a plane transverse to the said axis. The longitudinal effective mass, ml, is usually much larger than its counterparts mt. The DOS effective mass mae for electrons in the CB minima a ¼ G, X or L is given by 2=3

1=3

mae ¼ N 2=3 mta mla

ð7:3Þ

where N is the number of equivalent a minima (N ¼ 1 for the G minimum, N ¼ 3 for the X minima and N ¼ 4 for the L minima). The DOS mass can be used for DOS calculations. The conductivity effective mass mac , which can be used for conductivity or mobility calculations, is written as mac ¼

3mta mla mta þ 2mla

ð7:4Þ

Since mtG ¼ mlG, we have the relationship mGe ¼ mGc at the a ¼ G minimum. In hexagonal semiconductors, the CB electron has an ellipsoidal constant-energy surface, not a spherical surface, even at the zone center (G)

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

230

PROPERTIES OF SEMICONDUCTOR ALLOYS

jj m? e mx ¼ my 6¼ mz me

ð7:5Þ

Thus, mGe 6¼ mGc holds in such anisotropic semiconductors, but its difference is very small. We summarize in Table 7.1 the G-valley electron effective mass mGe for a number of cubic group-IV, III–V and II–VI semiconductors. Table 7.2 also summarizes the G-valley electron effective masses for some wurtzite III–V and II–VI semiconductors. The mGe values for InN, BeSe and BeTe in Table 7.1 and those for InN, BeO, BeSe and CdTe in Table 7.2 are obtained using the mGe versus E0 relationships described in Section 7.1.2 of Adachi [1]. The InN values in Table 7.2 are taken from Hofmann et al. [2]. The electron effective masses in the X (D) and L minima for some cubic group-IVand III–V semiconductors are listed in Table 7.3. The corresponding DOS and conductivity masses are listed in Table 7.4.

7.1.2 Hole Effective Mass The effective Hamiltonian is generally derived from a kp theory or from the theory of invariants developed by Bir and Pikus. The effective Hamiltonians for the CB and VB in the Table 7.1 Electron effective mass mGe for some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

BN (zb) BP (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

mGe /m0 0.36–2.030a 0.188a 0.038 0.058b 0.449a

System

Material

II–VI

BeSe (zb) BeTe (zb) MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

0.752a 0.150a 0.0499a 0.26a 0.220a 0.124 0.14 0.15 0.114 0.067 0.039 0.03a 0.07927 0.024 0.013

Calculated or estimated The sign is chosen positive for a normal band structure like that of Ge c The sign is chosen positive for a normal band structure like that of CdTe a b

mGe /m0 0.28a 0.21a 0.35a 0.225a 0.20a 0.17a 0.20 0.137 0.117 0.21 0.14a 0.112 0.090 0.006a,c 0.042a,c 0.028c

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

231

k

G Table 7.2 G-valley electron effective masses, m? e , me and me , for some wurtzite III–V and II–VI G ?2 k 1=3 semiconductors. me ¼ ðme me Þ : DOS effective mass jj

System

Material

m? e /m0

me /m0

mGe /m0

III–V

AlN GaN InN

0.29a 0.21 0.047

0.30a 0.22 0.039

0.29–0.45 (0.29a) 0.21 0.044

II–VI

BeO MgSe ZnO ZnS CdS CdSe CdTe

a

0.28 0.150 0.127

0.7a 0.3a 0.234 0.28 0.151 0.125 0.11a

0.28 0.152 0.122

Calculated or estimated

zinc-blende- and wurtzite-type semiconductors are shown in Section 6.2.1 of Adachi [1]. The expressions for the hole effective masses in terms of the Luttingers VB parameters g (cubic) and A (hexagonal) have been described in Section 7.3.1 of Adachi [1]. The g and A values for some cubic and wurtzite semiconductors are summarized in Tables 7.5 and 7.6, respectively. Table 7.7 also lists the effective HH and LH band masses, Table 7.3 Electron effective mass in the X (D) and L minima for some cubic group-IV and III–V semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb)

a

Theoretical

mtX/m0

X

L

mlX/m0

mtL/m0

mlL/m0

0.36 0.1905 0.29 0.086a 0.25

1.4 0.9163 1.35 0.89a 0.67

0.130a 0.081 0.075a

1.418a 1.61 1.478a

0.23a 0.204a 0.32a 0.212a 0.19 0.21 0.30a 0.252 0.23 0.33a 0.34a 0.28a

0.94a 1.125a 0.52a 3.67a 1.1 1.50 0.58a 6.9 1.3 1.30a 1.26a 1.32a

0.15a 0.20a

1.32a 1.82a

0.150a 0.0754 0.085 0.13a 0.12a

1.184a 1.9 1.4 1.64a 3.57a

232

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.4 Electron DOS mass mX;L and conductivity mass mX;L in the X and L minima for some cubic e c group-IV and III–V semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

Density-of-states mass mX e /m0

mLe /m0

mX c /m0

mLc /m0

0.73 0.553 0.51a

0.48 0.259 0.39 0.12a 0.32

0.19 0.119 0.11a

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

1.18 0.669 1.01 0.39a 0.72

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb)

0.76a 0.75a 0.78a 1.14a 0.71 0.84 0.78a 1.58 0.85 1.08a 1.09a 0.98a

a

Conductivity mass

0.78 1.05a 0.75a 0.56 0.54 0.76a 0.94a

0.31a 0.28a 0.37a 0.31a 0.26a 0.29 0.36a 0.37 0.32 0.44a 0.45a 0.38a

0.21a 0.28a 0.21a 0.11 0.12 0.19a 0.18a

Theoretical

mHH and mLH, along the [001] and [111] directions for some cubic semiconductors. The DOS HH ðmHH* Þ, averaged LH ðmLH* Þ and SO split-off hole effective masses (mSO) are summarized in Table 7.8. The c-InN g values in Table 7.5 are taken from Fritsch et al. [3].

7.1.3 Interpolation Scheme Let us consider a linear interpolation representation for the composition dependence of the effective mass m(x) for a semiconductor alloy AxB1x (AxB1xC). The simplest linear interpolation scheme is the use of the equation mAB ðxÞ ¼ xmA þ ð1xÞmB

ð7:6Þ

where mA and mB represent the masses of elemental (binary) semiconductors A (AC) and B (BC), respectively. If any material parameter can be given by a specific expression owing to some physical basis, it is natural to consider that the corresponding interpolation scheme may also obey this specific expression. The effective mass representation can then be written as 1 x 1x ¼ þ mAB ðxÞ mA mB

ð7:7Þ

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

233

Table 7.5 Luttingers VB parameter gi for some cubic group-IV, III–V and II–VI semiconductors (in h2/2m0). d ¼ diamond; zb ¼ zinc-blende System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

BN (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

II–VI

MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

a

g1

g2

g3

4.24 4.285 13.38 15.0 2.817

0.82 0.339 4.24 11.5 0.508

1.71 1.446 5.69 8.6 0.860

1.92a 1.73a 3.47a 3.76a 4.15a 2.84a 4.04 7.10 13.3 5.381a 5.33 20.4 36.3 2.62a 2.84a 3.21a 1.77a 3.94 3.96 4.11a 5.51a 4.14 41.28a 25.96a 15.6

0.02a 0.43a 0.06a 0.90a 1.01a 0.82a 0.53 2.02 4.4 2.294a 1.57 8.3 16.1 0.38a 0.43a 0.52a 0.30a 1.00 0.86 0.77a 1.24a 1.09 21.00a 13.69a 9.6

0.56a 0.65a 1.15a 1.42a 1.75a 1.12a 1.26 2.91 5.7 2.508a 2.11 9.1 17.2 0.91a 1.00a 1.15a 0.62a 1.52 1.39 1.53a 2.14a 1.62 20.73a 13.20a 8.6

Calculated or estimated

Similarly, for quaternary semiconductor alloys of types AxB1xCyD1y and AxByC1xyD (ABxCyD1xy) we obtain 1 xy xð1yÞ ð1xÞy ð1xÞð1yÞ ¼ þ þ þ mABCD ðx; yÞ mAC mAD mBC mBD

ð7:8aÞ

1 x y 1xy ¼ þ þ mABCD ðx; yÞ mAD mBD mCD

ð7:8bÞ

234

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.6 Theoretically obtained Luttingers VB parameter Ai for some wurtzite III–V and II–VI semiconductors A1

A2

A3

A4

A5

A6

|A7|

AlN GaN InN

4.15 6.87 9.15

0.39 0.68 0.66

3.76 6.27 8.50

1.61 2.98 4.52

1.76 3.05 4.47

2.07 4.25 5.74

0.10 0.23 0.33

ZnO ZnS CdS CdSe

3.78 4.58 5.92 10.2

0.44 0.53 0.70 0.76

3.45 4.14 5.37 9.53

1.63 2.34 1.82 3.2

1.68 2.34 1.82 3.2

2.23 3.69 1.36 2.31

0.025

System

Material

III–V

II–VI

Justification for Equation (7.7) is supported by the effective-mass transformation of the Schr€ odinger equation "

# h2 r2 X h2 r2 þ U ðrt Þ ! 2m0 2mAB ðxÞ r

ð7:9Þ

Figure 7.1 shows the effective HH band mass mHH as a function of x for AlxGa1xAs. The solid and dashed lines are obtained by introducing the GaAs (x ¼ 0) and AlAs values (x ¼ 1.0) from Table 7.7 into Equations (7.6) and (7.7), respectively. The dotted lines are obtained by introducing the linearly interpolated g values from Table 7.5 into the following equations (see Table 7.7 in Adachi [1]) mHH½001 ðxÞ ¼

1 g1 ðxÞ2g2 ðxÞ

ð7:10aÞ

mHH½111 ðxÞ ¼

1 g1 ðxÞ2g3 ðxÞ

ð7:10bÞ

It can be seen from Figure 7.1 that the dashed (Equation (7.7)) and dotted lines (Equation (7.10)) agree with each other.

7.2 GROUP-IV SEMICONDUCTOR ALLOY 7.2.1 CSi Binary Alloy The lowest CB valleys in diamond and Si are located at the X (D) point in the BZ [1]. Figure 7.2 X (a) plots the X-valley DOS and conductivity masses mX e and mc for CxSi1x. The solid and dashed lines show the linear interpolation results between diamond and Si listed in Table 7.4 using Equations (7.6) and (7.7), respectively. The solid circles also show the effective masses for 3C-SiC (x ¼ 0.5) taken from Table 7.4.

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

235

Table 7.7 HH and LH effective band masses, mHH and mLH, along the [001] and [111] directions for some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende; rs ¼ rocksalt System

mHH/m0

Material

smLH/m0

[0 0 1]

[1 1 1]

[0 0 1]

[1 1 1]

0.17 0.202 0.0457 0.026a 0.26

0.13 0.139 0.0404 0.031a 0.22

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

0.38 0.277 0.204 0.125 0.56

1.22 0.718 0.500 0.46 0.91

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

0.53b 0.375b 1.15b 0.30b 0.51b 0.47b 0.83b 0.34 0.33 0.22 1.261 0.46 0.26 0.24

1.25b 0.926b 2.33b 0.85b 1.09b 1.54b 1.67b 0.66 0.78 0.53 2.740 0.90 0.45 0.53

0.51b 0.150b 0.39b 0.28b 0.18b 0.16b 0.22b 0.20 0.090 0.045 0.100 0.12 0.027 0.015

0.33b 0.108b 0.33b 0.17b 0.15b 0.13b 0.20b 0.15 0.077 0.040 0.096 0.11 0.026 0.014

II–VI

MgO (rs) MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

1.60b 0.54b 0.51b 0.46b 0.85b 0.52 0.45 0.39b 0.33b 0.51 1.39b 0.70b 0.28

2.77b 1.25b 1.19b 1.10b 1.9b 1.11 0.85 0.95b 0.81b 1.11 5.56b 2.27b 0.63

0.35b 0.30b 0.27b 0.24b 0.42b 0.168 0.176 0.18b 0.13b 0.158 0.012b,c 0.019b,c 0.029c

0.31b 0.23b 0.21b 0.18b 0.33b 0.143 0.148 0.14b 0.10b 0.136 0.012b,c 0.019b,c 0.030c

The sign is chosen positive for a normal band structure like that of Ge Calculated or estimated c The sign is chosen positive for a normal band structure like that of CdTe a b

Figure 7.2(b) shows the HH and LH masses mHH and mLH along the [001] and [111] directions for CxSi1x. The solid lines represent the results calculated from Equation (7.6) using the diamond and Si values in Table 7.7. The 3C-SiC (x ¼ 0.5) values are also plotted in Figure 7.2(b). These values are calculated from a set of the Luttingers VB parameters derived by a five-level kp analysis [4]. Note that the HH and LH bands are anisotropic even in the

236

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.8 DOS HH ðmHH* Þ, averaged LH ðmLH* Þ and SO split-off hole effective masses (mSO) for some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende mHH* /m0

mLH* /m0

mSO/m0

0.78 0.528 0.345 0.029b 0.76

0.14 0.157 0.0427 0.19 0.24

0.394a 0.29 0.095 0.041 0.51

BN (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InN (zb) InP (zb) InAs (zb) InSb (zb)

0.99a

0.37a 0.0800a 0.35a 0.20a 0.16a 0.13 0.21a 0.17 0.083 0.043 0.098 0.11 0.026 0.014

0.52a 0.2220a 0.58a 0.29a 0.30a 0.317a 0.35a 0.34 0.165 0.12 0.186 0.21 0.14 0.10

MgS (zb) MgSe (zb) MgTe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

0.93a 0.88a 0.80a 1.42a 0.82 0.67 0.68a 0.57a 0.82 0.012a,c 0.019a,c 0.030c

System

Material

IV

Diamond (d) Si (d) Ge (d) Sn (d) 3C-SiC (zb)

III–V

II–VI

1.77a 0.63a 0.81a 0.9 1.27a 0.52 0.55 0.37 1.959 0.69 0.36 0.38

0.25a 0.23a 0.20a 0.36a 0.154 0.159 0.15a 0.11a 0.145 2.22a 1.07a 0.38

0.38a 0.35a 0.31a 0.56a 0.24 0.25 0.24a 0.18a 0.24 0.013a,c 0.031a 0.102a

Calculated or estimated The sign is chosen positive for a normal band structure like that of Ge c The sign is chosen positive for a normal band structure like that of CdTe a b

diamond- and zinc-blende-type semiconductors [1]. As can be easily seen from Figure 7.2(b), the anisotropic effect is most pronounced for the HH band, which has a strongly directionallydependent effective mass, with a larger mass along the [111] direction than along the [001] direction. Using the linear interpolation scheme, we can obtain the plausible effective mass values for 3C-SiC. Note, however, that it is very difficult to accurately measure the effective masses in semiconductors. This is especially true for the hole effective masses and also for the k 6¼ 0

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

237

1.2

Al xGa1-xAs

mHH/m0

1.0

[001] direction

0.8 0.6

[111] direction

0.4 0.2

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.1 Effective HH band mass mHH in the [001] and [111] directions as a function of x for AlxGa1xAs. The solid and dashed lines are calculated from Equations (7.6) and (7.7), respectively. The dotted lines are obtained by introducing the linearly interpolated g values in Table 7.5 into Equation (7.10)

(e.g. X and L valleys) electron masses in semiconductors (and even for the k ¼ 0 (G-valley) electron masses in wide band-gap semiconductors).

7.2.2 SiGe Binary Alloy The transition from a Ge-like CB edge (X (D) valley) to a Si-like edge (L valley) was verified by CR to occur between x ¼ 0.115 and 0.19 [5]. In SixGe1x, the CB edge mass ratios are predicted from Table 7.3 to be mlX/mtX ¼ 10.9 þ 9.0x (Ge-like) and mlL/mtL ¼ 4.8 0.1x (Si-like). Fink and Braunstein [5] carried out CR measurements on the CB of SiGe alloy at 891 GHz (337 mm) using an IR laser. The IR laser enabled measurements of the longitudinal and transverse effective masses to within 4 at% of each side of the alloy composition at which the CB edge switches from the [111] to the [001] direction (15 at% Si in Ge). The measured mass 1.4

1.5

(a)

mHH mLH

1.2

1.0 m eX

0.8 0.6

3C-SiC mcX

0.4

0.9 3C-SiC

0.6 [111]

[001]

0.3

0.2 0

(b)

mHH, mLH (1/m0)

m Xe , m Xc (1/m0)

1.2

CxSi1-x

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

X Figure 7.2 (a) X-valley DOS and conductivity masses mX e and mc for CxSi1x. The solid and dashed lines represent the linear interpolation results derived from Equations (7.6) and (7.7), respectively. The solid circles show the effective masses for 3C-SiC (x ¼ 0.5) taken from Table 7.4. (b) Effective HH and LH band masses mHH and mLH in the [001] and [111] directions for CxSi1x. The solid lines represent the linear interpolation results using Equation (7.6)

238

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.2

0.6 L-X (Δ) crossing m eX

0.8 0.6

m Le

0.4

m Xc Ge-like CB

0.2

(b)

0.5 * , m* , m mHH LH SO (1/m0)

1.0 meX(L) , mX(L) (1/m0) c

(a)

0

0.3 0.2 0.1

0.2 0.4 0.6 0.8 1.0 x

m*HH

0.4

m cL

0

SixGe1-x

0 0

mSO m*LH

0.2 0.4 0.6 0.8 1.0 x

Figure 7.3 (a) X- and L-valley DOS and conductivity masses mX;L and mX;L for SixGe1x. (b) DOS HH e c * * ðmHH Þ, averaged LH ðmLH Þ and SO split-off hole effective masses (mSO) for SixGe1x. The solid lines in (a) and (b) are calculated from Equation (7.6). The dashed line in (a) indicates the CB L–X (D) crossing composition xc 0.15

did not appear to change from their values in the pure constituents, although only the transverse mass of the [111], Ge-like minimum could be measured with reliable accuracy. More recent CR measurements on high-mobility 2D electron gas in strained Si0.94Ge0.06 showed an in-plane mass of 0.193m0 [6], in good agreement with the expectations of Table 7.3. The X- and L-valley DOS and conductivity masses mX;L and mX;L for SixGe1x calculated from Equation (7.6) are e c shown in Figure 7.3(a). Experimental hole masses based on CR are available from measurements of 2D samples for pseudomorphic SixGe1x channels on Si [7]. The results gave insight into the complexity of the VB structure. The DOS HH (mHH ), averaged LH (mLH ) and SO split-off hole effective masses (mSO) for SixGe1x calculated from Equation (7.6) using the Si and Ge values in Table 7.8 are shown in Figure 7.3(b).

7.3 III–V SEMICONDUCTOR TERNARY ALLOY 7.3.1 (III, III)–N Alloy Unfortunately, there is no experimental information on the carrier effective masses in III–N alloys. This necessitates the use of some type of interpolation scheme. The G-valley electron mass mGe versus composition x for c- and w-(III, III)–N ternaries are shown in Figure 7.4. Equation (7.6) is used as the linear interpolation expression. The corresponding endpoint binary data are taken from Tables 7.1 and 7.2.

7.3.2 (III, III)P Alloy Figure 7.5 shows the G-valley electron mass mGe for some P-based ternaries. No experimental determinations of the effective masses in AlxGa1xP and AlxIn1xP appear to be available. Therefore, the electron effective masses mGe in Figure 7.5 were obtained from Equation (7.6). The mGe mass in a random Ga0.5In0.5P alloy was determined to be (0.092 0.003)m0 by

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES 0.30

239

0.4

(a) c-(III, III)-N

(b) w-(III, III)-N

0.25

0.15

meΓ /m0

meΓ /m0

0.3

AlxGa1-xN

0.20

AlxIn1-xN

AlxGa1-xN

0.2

AlxIn1-xN

0.10 GaxIn1-xN

GaxIn1-xN

0.1

0.05 0

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.4 G-valley electron effective mass mGe versus x for (a) c- and (b) w-(III, III)–N alloys. The solid lines are calculated from Equation (7.6)

Emanuelsson et al. [8]. This value is somewhat lower than the linearly interpolated value obtained using Equation (7.6), but is in reasonable agreement with that obtained from Equation (7.7). The quadratic least-squares fit of the x ¼ 0.5 and endpoint data gives a bowing parameter of c ¼ 0.01854m0 (heavy solid line, see also Table 7.9). Emanuelsson et al. [8] found the G-valley electron mass in an ordered Ga0.5In0.5P alloy to be (0.088 0.003)m0, which was slightly smaller than the random alloy value (0.092m0).

7.3.3 (III, III)As Alloy (a) AlGaAs An important description of the carrier effective masses in semiconductors was presented by Adachi [9,10] who reviewed many carried out on GaAs, AlAs and AlxGa1xAs. We have already shown in Figure 7.1 the HH masses mHH in the [001] and [111] directions for 0.24 0.21

meΓ /m0

0.18

AlxGa1-xP

0.15 AlxIn1-xP

0.12 0.09 0.06

GaxIn1-xP

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.5 G-valley electron effective mass mGe versus x for (III, III)–P alloys obtained from the linear interpolation scheme in Equation (7.6) (solid lines). The solid circle represents the CR data for a random Ga0.5In0.5P alloy obtained by Emanuelsson et al. [8]. The heavy solid line shows the quadratic least-squares fit of the endpoint binary data and Emanuelssons data (see Table 7.9)

240

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.9 G-valley electron effective mass mGe determined experimentally for some cubic III–V semiconductor alloys Alloy

mGe /m0

Remark

Gax In1xP AlxGa1xAs Alx In1xAs Gax In1xAs Gax In1xSb GaNx As1x GaPx As1x GaAsxSb1x InPx As1x Inx As1xSb Gax In1xPyAs1y /InP (AlxGa1x)0.48In0.52As/InP

0.07927 þ 0.01619x þ 0.01854x2 0.067 þ 0.057x 0.024 þ 0.088x þ 0.012x2 0.024 þ 0.035x þ 0.008x2 0.013 þ 0.016x þ 0.010x2 0.0067 þ 0.047x (x in at%) 0.067 þ 0.047x 0.039 þ 0.014x þ 0.014x2 0.02400 þ 0.05572x 0.013 0.016x þ 0.027x2 0.04084 þ 0.03384y þ 0.00459y2 0.043 þ 0.031x

0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 x 2 at% 0 x 1.0 0 x 1.0 0 x 1.0 0 x 1.0 0 y 1.0 0 x 1.0

AlxGa1xAs. The G-, X- and L-valley electron conductivity masses mGe , mcX and mcL for AlxGa1xAs have been plotted in Figure 7.6(a). The solid lines represent the linear interpolation results of Equation (7.6) using the endpoint binary data in Tables 7.1 and 7.4. The solid circles show the experimental mGe data taken from Adachi [10]. The corresponding linear least-squares fit is represented by the heavy solid line (see also Table 7.9). Figure 7.6(b) plots the cyclotron HH and LH masses mHc and mLc in the [001] direction as a function of x for AlxGa1xAs. The experimental data are taken from Adachi [10]. The cyclotron masses mHc and mLc result from averaging the band effective masses in Equation (47) in Hensel and Suzuki [11]. The solid lines in Figure 7.6(b) show the linear interpolation results between AlAs and GaAs using Equation (7.6), while the heavy solid lines represent the results 1.0 m eX

0.6

meΓ /m0

0.10

0.4 mcX

0.08 meΓ

0.06 0.04 0.02

0

0.2 0

0.7 0.6

mHc

0.20

0.5 mLc

0.4 0.3

Γ-X crossing

0.2

AlxGa1-xAs

0.1

0.2 0.4 0.6 0.8 1.0 x

0.25 (b)

0

0.15 0.10

mLc /m0

0.12

0.8

mHc/m0

(a)

meX, mcX (1/m0)

0.14

0.05 [001] direction

0

0 0.2 0.4 0.6 0.8 1.0 x

X Figure 7.6 (a) G- and X-valley electron effective masses mGe , mX e and mc for AlxGa1xAs. The solid lines show the linearly interpolated results using Equation (7.6). The heavy solid line represents the linear least-squares fit (see Table 7.9). The dashed line indicates the CB G–X crossing composition xc 0.4. (b) Cyclotron HH and LH masses mHc and mLc in the [001] direction for AlxGa1xAs. The solid lines show the linear interpolation results using Equation (7.6). The heavy solid lines are obtained by introducing the linearly interpolated g values into Equation (47) of Hensel and Suzuki [11]. The experimental data in (a) and (b) are taken from Adachi [10] (solid circles)

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

241

calculated by introducing the linearly interpolated g values (Equation (7.6)) into Equation (47) of Hensel and Suzuki [11]. (b) AlInAs Matyas and Karoza [12] determined the G-valley electron mass mGe from a plasma resonance minimum in the IR reflectance spectra for bulk AlxIn1xAs alloy. Their results (solid circles), X together with the linearly interpolated mGe , mX e and mc using Equation (7.6) (solid lines) are shown in Figure 7.7 The experimental mGe data for x > 0.08 are considerably larger than the linearly interpolated values. Similarly, Wright et al. [13] obtained from optically detected CR a considerably larger value of mGe ¼ (0.10 0.01)m0 for Al0.48In0.52As grown by MBE on InP. On the other hand, Cury et al. [14] measured a much smaller mass of mGe ¼ 0.069m0 which is only a little lower than the linearly interpolated value obtained using Equation (7.6) (0.072m0). The smaller result is supported by the optically detected CR measurements by Chen et al. [15]. The heavy solid line in Figure 7.7 shows the quadratic least-squares fit of the endpoint and Curys data (see also Table 7.9). 1.0 meX

0.12

0.6

AlxIn1-xAs

0.10 meΓ /m0

0.8

0.4

0.08

0.2

mcX

meX , mcX (1/m0)

0.14

0

0.06

meΓ

0.04 Γ-X crossing

0.02 0

0

0.2

0.4

0.6

0.8

1.0

x X Figure 7.7 G- and X-valley electron effective masses mGe , mX e and mc for AlxIn1xAs. The solid and open circles represent the experimental data taken from Matyas and Karoza [12] and Cury et al. [14], respectively. The solid lines show the linear interpolation results using Equation (7.6). The heavy solid line shows the quadratic least-squares fit of the endpoint binary data and Curys data (see Table 7.9). The dashed line indicates the CB G–X crossing composition xc 0.63

(c) GaInAs The G-valley electron mass mGe in GaxIn1xAs has been measured by a number of authors [16–20]. These results are shown in Figure 7.8(a). The solid and dashed lines represent the linear interpolation results of Equations (7.6) and (7.7) using the endpoint binary data in Table 7.1, respectively. The heavy solid line shows the quadratic least-squares fit of the experimental data, yielding a small bowing value of c ¼ 0.008m0 (Table 7.9). A set of the Luttingers VB parameters g for GaxIn1xAs have been measured by several authors [21–23]. Traynor et al. [23] observed a significant bowing in k defined by 1 2 2 k ¼ g1 þ g2 þ g3 3 3 3

ð7:11Þ

242

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.08 0.07

8 Gax In1-x As

(a)

6

κ (ħ2/2m0)

meΓ/m0

0.06 0.05 0.04 0.03

5 4 3 2

0.02 0.01 0

(b)

7

1 0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.8 (a) G-valley electron effective mass mGe for GaxIn1xAs. The solid and dashed lines show the linear interpolation results of Equations (7.6) and (7.7), respectively. The heavy solid line represents the quadratic least-squares fit (see Table 7.9). (b) Plots of k values for GaxIn1xAs. The symbols represent the experimental data taken from various sources (see text). The solid and dashed lines are obtained by introducing the linearly interpolated g values of Equations (7.6) and (7.7) into Equation (7.11), respectively

which is a parameter introduced by Luttinger and necessary to describe the magnetic levels, although it is not measured in classical CR experiments. The k values reported by Traynor et al. [23] are plotted against x ¼ 0.08 and 0.11 in Figure 7.8(b) (open triangles), together with those obtained from the Luttingers VB parameters by Alavi et al. [21] for x ¼ 0.47 (solid circle) and Warburton et al. [22] for x ¼ 0.82 (open circle). The solid and dashed lines in Figure 7.8(b) show the k values obtained by introducing the linearly interpolated g values from Equations (7.6) and (7.7) into Equation (7.11), respectively.

7.3.4 (III, III)Sb Alloy No experimental data are available for the effective masses in AlxGa1xSb and AlxIn1xSb. It can be expect however, that the G-valley mass mGe will be satisfactorily represented by the linear interpolation scheme. That is, any nonlinearity in the composition dependence of the effective mass stems entirely from the bowing of the energy band gap (see Figure 7.26). Very little strong bowing in the E0 gap has been observed experimentally for AlxGa1xSb and AlxIn1xSb (Figures 6.25 and 6.26). Figure 7.9(a) shows the G-valley electron mass mGe in GaxIn1xSb measured by Aubin et al. [24]. The solid and dashed lines are obtained by introducing the InSb (x ¼ 0) and GaSb values (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. The heavy solid line represents the quadratic least-squares fit of the experimental data. The VB structure of GaxIn1xSb was investigated by Roth and Fortin [25] using an interband magneto-optical technique. All the fundamental band parameters obtained by these authors exhibited a nonlinear dependence on x. The HH and LH band masses mHH and mLH in the [001] direction for GaxIn1xSb have been plotted in Figure 7.9(b) as examples. These plots are obtained by introducing the nonlinear g values into the expressions shown in Table 7.7 of Adachi [1] (see also an expression for mHH in Equation (7.10a)). The results can be expressed as

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES 0.045 GaxIn1-xSb

0.05

0.5

0.04

[001] direction

0.4

0.030

m HH/m0

meΓ/m0

0.035

0.025

0.015 0.010 0

0.02

mHH

0.2

0.020

0.03

mLH

0.3

0.01

0.1 (a)

0.2 0.4 0.6 0.8 1.0 x

mLH/m0

0.040

0.6

243

(b)

0

0

0 0.2 0.4 0.6 0.8 1.0 x

Figure 7.9 (a) G-valley electron effective mass mGe in GaxIn1xSb. The experimental data are taken from Aubin et al. [24]. The solid and dashed lines are obtained from Equations (7.6) and (7.7), respectively. The heavy solid line shows the quadratic least-squares fit (see Table 7.9). (b) Effective HH and LH band masses mHH and mLH in the [001] direction for GaxIn1xSb. These plots are obtained by introducing the Luttingers VB parameters g determined experimentally by Roth and Fortin [25] into the expressions in Table 7.7 of Adachi [1] (see also Equation (7.12))

mHH ¼ 0:246 m0

ð7:12aÞ

mLH ðxÞ ¼ 0:017 þ 0:009x þ 0:015x2 m0

ð7:12bÞ

7.3.5 Dilute-nitride III–(V, V) Alloy (a) Ga(N, V) alloy The conductivity masses at the lowest direct and indirect conduction minima of GaP are mGe ¼ 0.114m0 (Table 7.1) and mXc ¼ 0.37m0 (Table 7.4), respectively. A large CB effective mass of 0.9m0 has been estimated by analyzing PL spectra for GaNxP1x/GaP MQWs of various well thicknesses [26]. The results may indicate a mixing of the G- and X-valley wavefunctions in the CB. The electron effective mass in dilute-nitride GaNxAs1x has been measured using various techniques, such as optically detected CR [27], PR [28] and magneto-PL measurements [29–31]. These results have been plotted in Figure 7.10. Since the band structure of dilute nitrides is still unclear, let us use a new symbol m*e for the free-electron effective mass. There is a large scatter in m*e . The solid line represents the linear least-squares fit of these data (see also Table 7.9). Zhang and Mascarenhas [32] investigated quantum-confinement phenomena in GaNxAs1x/GaAs QWs (0.009 x 0.045) using an ER technique. They demonstrated formation of an impurity band due to heavy N doping and the quantum confinement of an electron belonging to such an impurity band. The resulting electron effective masses are much larger than those shown in Figure 7.10 (e.g. m*e 0.55m0 at x ¼ 0.009 and 0.4m0 at x ¼ 0.023). The extremely large m*e value with N incorporation and its subsequent decrease can be expected to be a result of the impurity band formation.

244

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.30 0.25

GaNxAs1-x

0.08

0.15 meΓ/m0

meΓ/m0

0.20

0.10 0.05 0 0

0.06 0.04 0.02 0

1

2 x (at%)

3

0.2 0.4 0.6 x (at%)

4

Figure 7.10 Electron effective mass m*e in dilute-nitride GaNxAs1x. The solid line represents the linear least-squares fit (see Table 7.9). The inset shows the experimental results of Young et al. [33] for x from 0 up to 0.4 at%. The solid line in the inset also shows the quadratic least-squares fit of Equation (7.13)

In contrast, by analyzing carrier transport properties Young et al. [33] observed a decrease in m*e with increasing x from 0 up to 0.4 at% in GaNxAs1x. Their results are reproduced in the inset of Figure 7.10. The solid line shows the quadratic least-squares fit of these data (x in at%) m*ðxÞ e ¼ 0:0670:194x þ 0:246x2 m0

ð7:13Þ

The traditional kp theory predicts that the CB mass should decrease with decreasing bandgap energy [1] (Figure 7.26). We have shown that adding N to GaAs reduces its band-gap energy considerably (Figure 6.29), so this effect alone may be expected to reduce the effective mass. On the other hand, any effect of N incorporation on the CB wavefunction admixture will increase the electron effective mass [34]. Young et al. [33] considered that their samples lay at the limit of dilute alloy where there are minor perturbations of the CB. The observed m*e reduction is thus thought to be due to the band-gap reduction. The large increase in m*e observed in the intermediate or higher N concentration region [27–31] is due to the mixing effect of the CB states (G, X and L). The effect of N incorporation on the electron effective mass is more subtle and it may represent a more stringent test for the validity of different theoretical models aimed at explaining the puzzling effects of N in various III–V semiconductors [34]. Unfortunately, the experimental m*e data reported do not show a common and clear trend with increasing N concentration, as can be seen from Figure 7.10. (b) In(N, V) alloy The electron effective mass m*e in dilute-nitride InNxAs1x has been measured by several authors [35–37]. Figure 7.11 plots the results obtained by these authors (solid circles: Huang et al. [35]; open circle: Hang et al. [36]; open triangles: Shih et al. [37]). The heavy solid line shows the quadratic least-squares fit of these data (x in at%)

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

245

0.4

meΓ/m0

0.3

InNx As1-x

0.2 0.1 0 0

1

2

3

4

x (at%)

Figure 7.11 Electron effective mass m*e in dilute-nitride InNxAs1x. The solid and dashed lines are calculated by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. Note that these lines completely overlap in the region of x 4 at%. The heavy solid line shows the quadratic least-squares fit of Equation (7.14)

m*e ðxÞ ¼ 0:0240:018x þ 0:029x2 m0

ð7:14Þ

The solid and dashed lines are obtained by introducing the InAs (x ¼ 0) and c-InN values (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. The effective mass m*e in dilute-nitride InNxSb1x has been measured by Murdin et al. [38] using the CR technique. The experimental m*e value for x ¼ 0.044 at 5.53 mm exciting laser wavelength was 0.044, which was compared with 0.033 for InSb (x ¼ 0) at the same wavelength. Since N incorporation mainly affects the CB states [34], the dilute-nitride hole effective masses can be compared with those of the hole masses in the nitride-free III–V host semiconductors, such as GaP, GaAs, InAs and InSb.

7.3.6 Al(V, V) Alloy No experimental data are available on the effective masses of Al-based ternary alloys. Therefore, the linearly interpolated mGe values for AlPxAs1x, AlPxSb1x and AlAsxSb1x using Equation (7.6) are shown in Figure 7.12. The endpoint binary masses are taken from Table 7.1.

7.3.7 Ga(V, V) Alloy (a) GaPAs Figure 7.13(a) shows the G-valley electron effective mass mGe in GaPxAs1x measured by Wetzer et al. [39] using an optical detection CR technique. The solid and dashed lines represent the linear interpolation results obtained by introducing the GaAs (x ¼ 0) and GaP values (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. There is a tendency for upward bowing in the experimental mGe versus x plots; however, the same alloy showed a weak downward bowing in E0 (Figure 6.33). It can, therefore, be concluded that GaPxAs1x has an almost linear dependence of mGe on x. The resulting expression is given in Table 7.9.

246

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.24 0.21 meΓ/m0

0.18

AlPxAs1-x AlPxSb1-x

0.15 0.12

AlAsxSb1-x

0.09 0.06

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.12 G-valley electron effective mass mGe versus x for Al(V, V) alloys obtained from the linear interpolation scheme of Equation (7.6)

(b) GaAsSb Filion and Fortin [40] determined the G-valley electron effective mass mGe in GaAsxSb1x by measuring intrinsic photoconductivity under magnetic fields of up to 65 kG. The data they obtained for mGe , together with the linearly interpolated results using Equations (7.6) and (7.7) are shown in Figure 7.13(b). The result calculated using Equation (7.7), shown by the dashed line, explains the peculiar experimental data very well and can be approximated by the quadratic expression given in Table 7.9.

7.3.8 In(V, V) Alloy (a) InPAs The electron effective mass mGe in InPxAs1x has been measured by various authors [41–45]. The solid line in Figure 7.14 represents the linear least-squares fit of these data (see Table 7.9). 0.14

0.08 (a) GaPxAs1-x

(b) GaAsxSb1-x

0.07

0.12

meΓ/m0

meΓ/m0

0.06 0.10 0.08

0.05 0.04

0.06 0.04 0

0.03 0.2 0.4 0.6 0.8 1.0 x

0.02

0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.13 G-valley electron effective mass mGe versus x for (a) GaPxAs1x and (b) GaAsxSb1x. The experimental data in (a) are taken from Wetzel et al. [39] and in (b) from Filion and Fortin [40] (solid circles). The solid and dashed lines are obtained by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. The expressions used to obtain these lines are listed in Table 7.9

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

247

0.10

meΓ/m0

0.08

InPxAs1-x

0.06 0.04 0.02 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.14 G-valley electron effective mass mGe in InPxAs1x. The solid line represents the linear least-squares fit (see Table 7.9)

(b) InAsSb The electron effective mass mGe in InAsxSb1x obtained from Thomas and Woolley [46] is shown in Figure 7.15(a). The solid and dashed lines represent the linear interpolation results obtained by introducing the InSb (x ¼ 0) and InAs data (x ¼ 1.0) in Table 7.1 into Equations (7.6) and (7.7), respectively. The heavy solid line also shows the quadratic least-squares fit of the experimental data. The bowing parameter c obtained from this fit is 0.027m0, which is much larger than the endpoint values mGe ¼ 0.013m0 (InSb) and 0.024m0 (InAs). The resulting mGe versus x curve exhibits considerably large downward bowing, as shown in Figure 7.15(a). A full set of the Luttingers VB parameters for InAsxSb1x have been determined by Smith et al. [47] from interband magnetoabsorption measurements. The results they obtained have been plotted in Figure 7.15(b). These parameters show almost linear dependence on x.

0.030

40 Inx As1-xSb

32

0.020

γi (ħ2/2m0)

meΓ/m0

(b)

36

(a)

0.025

0.015

28

γ1

24 20 16

0.010

γ2

12 0.005 0

0.2 0.4 0.6 0.8 1.0 x

8

0

γ3

0.2 0.4 0.6 0.8 1.0 x

Figure 7.15 (a) G-valley electron effective mass mGe in InAsxSb1x. The experimental data are taken from Thomas and Woolley [46]. The solid and dashed lines are obtained by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. The heavy solid line shows the quadratic leastsquares fit (see Table 7.9). (b) Luttingers VB parameters for InAsxSb1x determined by Smith et al. [47]

248

PROPERTIES OF SEMICONDUCTOR ALLOYS

7.4 III–V SEMICONDUCTOR QUATERNARY ALLOY 7.4.1 Dilute-nitride Quaternary Alloy As mentioned in Section 7.3.5, the electron effective mass m*e in dilute-nitride III–V ternaries is usually larger than the electron effective mass mGe in the host materials, possibly due to the interaction of the CB with N-related resonant states. The same conclusion can be drawn for dilutenitride III–V quaternaries. The electron effective mass m*e in dilute-nitride GaxIn1xNyAs1y obtained by Pan et al. [48] and Heroux et al. [49] is shown in Figure 7.16. These data show a clear increase in m*e with increasing N concentration. A number of groups also observed an increase in the electron effective mass by incorporating N atoms into GaxIn1xAs [50–54]. 0.12

GaxIn1-xNyAs1-y me*/m0

0.10 0.08 0.06 0.04

x=0.7 0.86 0

0.5

1.0

1.5

2.0

N (at%)

Figure 7.16 Electron effective mass m*e in dilute-nitride GaxIn1xNyAs1y reported by Pan et al. [48] (solid circles) and Herouz et al. [49] (open circles)

Polimeni et al. [55] found that there was dependence of the in-plane hole effective masses in GaxIn1xNyAs1y QWs on the In concentration by PL measurements after picosecond excitation and under a magnetic field B. These results suggest that the dilute-nitride hole effective masses are nearly the same as those for nitride-free GaxIn1xAs host semiconductor. This agrees with the fact that N incorporation mainly affects the CB states [34].

7.4.2 (III, III)–(V, V) Alloy (a) GaInPAs Adachi [56] has reviewed the carrier effective masses in GaxIn1xPyAs1y. The G-valley electron effective mass mGe versus y for GaxIn1xPyAs1y/InP has been plotted in Figure 7.17(a). The solid and dashed lines represent the linear interpolation results obtained from Equations (A.6) and (7.8) respectively, using the binary data in Table 7.1. The solid circles show the experimental data taken from Adachi [56]. The corresponding quadratic least-squares fit is given by the heavy solid line (see also Table 7.9). The LH effective mass in GaxIn1xPyAs1y/InP versus y is plotted in Figure 7.17(b). The experimental data are taken from Adachi [56]. The solid and dashed lines represent the linear interpolation results obtained from Equations (A.6) and (7.8) respectively, using the binary data in Table 7.7. The heavy solid line shows the quadratic best-fit expression

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES 0.10

249

0.14 GaxIn1-xPyAs1-y /InP

0.12

0.08 mLH /m0

meΓ/m0

0.10 0.06

0.08 0.06

0.04 0.04

(a) 0.02 0

(b)

0.2 0.4 0.6 0.8 1.0 y

0.02 0

0.2 0.4 0.6 0.8 1.0 y

Figure 7.17 (a) G-valley electron effective mass mGe and (b) LH effective mass mLH versus y for GaxIn1xPyAs1y /InP. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively. The solid circles show the experimental data taken from Adachi [56]. The heavy solid lines represent the quadratic least-squares fit in Table 7.9 ðmGe Þ and the result obtained using Equation (7.15) (mLH). The open squares correspond to the InP (y ¼ 1.0) data

mLH ðyÞ ¼ 0:05 þ 0:04y þ 0:03y2 m0

ð7:15Þ

(b) GaInAsSb No experimental data on the carrier effective masses in GaxIn1xAsySb1y has been reported. The linearly interpolated mGe values for GaxIn1xAsySb1y lattice-matched to GaSb and InAs have therefore been plotted in Figure 7.18. The solid and dashed lines represent the linear interpolation results of Equations (A.6) and (7.8) respectively, using the binary data in 0.05

0.05

(a)

(b) 0.04 meΓ/m0

meΓ/m0

0.04

0.03

0.02

0.03

0.02 GaxIn1-xAsySb1-y /GaSb

0.01 0

0.2 0.4 0.6 0.8 1.0 x

Gax In1-x AsySb1-y /InAs

0.01 0

0.2 0.4 0.6 0.8 1.0 x

Figure 7.18 G-valley electron effective mass mGe versus x for (a) GaxIn1xAsySb1y /GaSb and (b) GaxIn1xAsySb1y/InAs. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively

250

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 7.1. The results of GaxIn1xPyAs1y / InP in Figure 7.17 support the use of Equation (A.6) for providing more plausible effective masses for III–V semiconductor alloys.

7.4.3 (III, III, III)–V Alloy (a) AlGaInP The electron effective mass mGe in (AlxGa1x)0.53In0.47P/GaAs has been measured by Emanuelsson et al. [8] using conventional and optically detected CR measurements. The result they obtained mGe /m0 ¼ 0.14 0.01 (x ¼ 0.3) is shown in Figure 7.19, together with those calculated from Equations (A.6) and (7.8) using the binary data in Table 7.1 (solid and dashed lines). The experimental data is found to be slightly larger than the interpolated value obtained using Equation (A.6) (solid line). This may be due to X-valley interactions (see Figure 6.49) and/or any effect of band nonparabolicity.

Figure 7.19 G-valley electron effective mass mGe versus x for (AlxGa1x)0.53In0.47P/GaAs. The solid circle represents the experimental data taken from Emanuelsson et al. [8]. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively

(b) AlGaInAs The G-valley electron effective mass mGe in (AlxGa1x)0.48In0.52As/InP has been measured by several authors [14,15,57,58]. Figure 7.20 shows these results (solid circles), together with those obtained from Equations (A.6) and (7.8) using the binary data in Table 7.1 (solid and dashed lines). The linear least-squares fit of the experimental data is also shown by the heavy solid line (see also Table 7.9). Equation (A.6) has been found to estimate mGe more reliably than Equation (7.8).

7.4.4 III–(V, V, V) Alloy Theelectron effective mass mGe in InPxAsySb1xy/InAs hasbeen measured byVoronina et al. [59] using various techniques, such as the Shubnikov–de Haas effect, Hall effect, magnetoresistance and photoconductivity. This result is plotted in Figure 7.21 (x ¼ 0.26, y ¼ 0.62). The solid and dashed lines show the linear interpolation results of Equations (A.6) and (7.8) respectively, using the binary data in Table 7.1. It can be seen that the experimental data is slightly smaller than the linearly interpolated value derived using Equation (A.6) (solid line).

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

251

0.09 (AlxGa1-x)0.48In0.52As/InP

0.08 meΓ /m0

0.07 0.06 0.05 0.04 0.03

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.20 G-valley electron effective mass mGe versus x for (AlxGa1x)0.48In0.52As/InP. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively. The heavy solid line shows the quadratic least-squares fit (see Table 7.9)

0.08

InPx AsySb1-x-y /InAs meΓ /m0

0.06 0.04 0.02 0

0

0.2

0.4

0.6

0.8

1.0

y

Figure 7.21 G-valley electron effective mass mGe versus x for InPxAsySb1xy/InAs. The solid circle represents the experimental data taken from Voronina et al. [59]. The solid and dashed lines are obtained by introducing the binary data into Equations (A.6) and (7.8), respectively

7.5 II–VI SEMICONDUCTOR ALLOY 7.5.1 (II, II)–VI Ternary Alloy Lu et al. [60] obtained the electron effective mass mGe in MgxZn1xO from analyzing the Burstein–Moss shift. The mass values they obtained are plotted in Figure 7.22(a). The electron effective mass increased with increasing x from 0.30m0 (x ¼ 0) to 0.49m0 (x ¼ 0.21). Note, however, that the ZnO (x ¼ 0) value is slightly larger than that estimated from the generalized mGe versus E0 relationship (0.23m0) [1]. Figure 7.22(b) shows the G-valley electron effective mass mGe in c-ZnxCd1xSe reported by Imanaka and Miura [61] (solid circle), Lo et al. [62] (open circle) and Ng et al. [63] (open triangles). We can see that the data of Lo et al. is considerably larger than that estimated from the linear interpolation scheme (solid and dashed lines). Shao et al. [64] also determined the mGe value in Zn0.80Cd0.20Se/ZnS0.06Se0.94 QW by Shubnikov–de Haas oscillations. The

252

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.8

0.16 (a) MgxZn1-xO

0.7

0.15

(b) c-ZnxCd1-xSe

wurtzite

0.14 rocksalt

0.5

meΓ/m0

meΓ/m0

0.6

0.4

0.13 0.12

mixed phase

0.3 0.2 0

0.11 0.10 0

0.2 0.4 0.6 0.8 1.0 x

0.2 0.4 0.6 0.8 1.0 x

Figure 7.22 (a) G-valley electron effective mass mGe in MgxZn1xO. The experimental data are taken from Lu et al. [60]. (b) G-valley electron effective mass mGe in c-ZnxCd1xSe. The experimental data are taken from Imanaka and Miura [61] (solid circle), Lo et al. [62] (open circle) and Ng et al. [63] (open triangles). The solid and dashed lines in (b) are obtained by introducing the endpoint binary data into Equations (7.6) and (7.7), respectively. The open squares in (a) and (b) show the endpoint binary data in Table 7.1

value they obtained, 0.17m0 (x ¼ 0.80) is, however, much larger than the endpoint binary data. The larger mGe value was considered to be due to the effect of a parallel conduction layer in the sample measured [64]. The Hg-based ternaries ZnxHg1xTe and CdxHg1xTe exhibit a semimetallic nature at low x compositions (E0 < 0 eV, see Figure 6.58). The corresponding CB electrons have a negative mass value. The G-valley electron effective masses mGe in ZnxHg1xTe and CdxHg1xTe are shown in Figure 7.23. The experimental data for ZnxHg1xTe are taken from Shneider and Tsiutsiura [65] and for CdxHg1xTe from Kim and Narita [66] (open triangles) and Laurenti 0.20

0.10 (a) ZnxHg1-xTe

0.15

0.08 0.06 meΓ/m0

meΓ/m0

0.10 0.05 0

T= 0 K 300 K

0.04 0.02 0

semimetallic

-0.05 -0.10

(b) CdxHg1-xTe

0

0.2 0.4 0.6 0.8 1.0 x

-0.02 -0.04 0

semimettalic

0.2 0.4 0.6 0.8 1.0

Figure 7.23 G-valley electron effective mass mGe in (a) ZnxHg1xTe and (b) CdxHg1xTe. The experimental data in (a) are taken from Shneider and Tsiutsiura [65] and in (b) from Kim and Narita [66] (at 4.2 K, open triangles) and Laurenti et al. [67] (at 0 K (solid circles) and 300 K (open circles)). The solid lines in (a) and (b) are obtained by introducing the endpoint binary data into Equation (7.6)

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

253

et al. [67] (T ¼ 0 K (solid circles), 300 K (open circles)). A large difference can be seen between the experimental and linearly interpolated values for ZnxHg1xTe. Note that the Hg-based alloys have positive and strongly x-dependent coefficients dE0/dT at high Hg concentrations (Figure 6.57). The semimetal/semiconductor crossing composition and free-electron concentration then show strong temperature dependence [67–69]. These facts make it difficult to accurately determine the electron effective mass at high Hg concentration. Note also that the lowest CB minimum in a semiconductor region is at the G6 state while that in a semimetal region is at the G8 state (i.e. the LH band in the cubic, zinc-blende semiconductors).

7.5.2 II–(VI, VI) Ternary Alloy The G-valley electron effective mass mGe in w-CdSxSe1x has been determined by analyzing optical absorption spectra using a kp method [70]. These results have been plotted in Figure 7.24. The solid line also shows the linear interpolation result obtained by introducing the endpoint binary data in Table 7.1 into Equation (7.6). 0.30

w-CdSxSe1-x

meΓ/m0

0.24 0.18 0.12 0.06 0 0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.24 G-valley electron effective mass mGe in w-CdSxSe1x. The experimental data are taken from Brodin et al. [70]. The solid line is obtained by introducing the endpoint binary data into Equation (7.6)

Brodin et al. [70] reported the x-dependent hole effective masses at the three VB states (G9, G7 and G7). All these hole masses and mGe (Figure 7.24) increased almost linearly from CdSe (x ¼ 0) to CdS (x ¼ 1.0).

7.5.3 (II, II)–(VI, VI) Quaternary Alloy No detailed experimental determinations of the electron or hole effective mass in II–VI quaternary alloys have been carried out. Therefore, the G-valley electron effective mass mGe in MgxZn1xSySe1y/GaAs obtained from the linear interpolation scheme is shown in Figure 7.25. The solid and dashed lines were obtained from Equations (A.6) and (7.8), respectively. The interpolated values show upward bowing. For example, the solid line can be expressed as mGe ðxÞ ¼ 0:14 þ 0:12x0:04x2 m0

ð7:16Þ

254

PROPERTIES OF SEMICONDUCTOR ALLOYS 0.30

Mgx Zn1-xSySe1-y /GaAs

meΓ/m0

0.25 0.20 0.15 0.10

0

0.2

0.4

0.6

0.8

1.0

x

Figure 7.25 G-valley electron effective mass mGe in MgxZn1xSySe1y/GaAs. The solid and dashed lines are calculated by introducing the binary data into Equations (A.6) and (7.8), respectively

7.6 CONCLUDING REMARKS 7.6.1 Composition Dependence The simple three-band kp theory gives m0 P2 2 1 P2 P2 0 ¼ 1 þ þ þ C / þ C

mGe 3 E0 E0 þ D0 E0 E0

ð7:17Þ

where P is the momentum matrix element relating the p-like VB to the s-like CB and C (C 0 ) is a correction for all higher-lying bands. Thus, the G-valley electron effective mass mGe is expected to be proportional to E0 (see Equations (7.8) and (7.9) in Adachi [1]). Figure 7.26 plots the E0 and mGe versus x for some cubic III–V ternaries. It can be seen that the smaller E0-gap material has a smaller mGe value, as predicted by Equation (7.17). The results in Sections 7.2–7.5 also indicate that linear interpolation (especially Equation (7.6) or Equation (A.6)) is an easy and effective means to obtain the electron and hole effective masses in semiconductor alloys.

7.6.2 External Perturbation Effect Like the G-point energy gaps (E0 and E0 þ D0 ), the electron and hole effective masses at the G point of non-alloyed semiconductors decrease with increasing temperature (T) and also increase with increasing pressure p [1]. The same tendency can be expected in semiconductor alloys. Laurenti et al. [67] observed that increasing T from 0 to 500 K leads to a gradual decrease in the mGe value of CdxHg1xTe for x 0.5. Similarly, Nicholas et al. [42] found that for InPxAs1x (0 x 1.0) the value of mGe was relatively constant from low T up to T 100 K and that further increases in T decreased mGe in an almost proportional manner. The change in the electron effective mass DmGe from T ¼ 0 to 300 K was less than 8%. The pressure dependence of the electron effective mass mGe in InPxAs1x has been measured by Torres and Stradling [44]. These results have been plotted in Figure 7.27. It can be seen that mGe increases almost linearly with increasing p. Similarly, an increase in mGe has been observed in Ga0.47In0.53As [71,72] and also in dilute-nitride GaxIn1xNyAs1y (m*e ) [73,74].

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

255

3.5 (a)

3.0

E0 (eV)

2.5 2.0 1.5 1.0 0.5 0 0.15 (b)

meΓ/m0

0.10

0.05

0 AlAs

GaAs

InAs x

InSb

GaSb

Figure 7.26 (a) Lowest direct gap (E0) at 300 K and (b) G-valley electron effective mass ðmGe Þ versus composition x for some III–V ternaries. The experimental data are plotted by the solid circles

6.4 InPx As1-x

meΓ /m×0 (x10-2)

6.0

x = 0.66

5.6 4.8 x = 0.31

4.4 4.0

x = 0.22

3.6 0

0.4

0.8

1.2

1.6

p (GPa)

Figure 7.27 Pressure dependence of mGe in InPxAs1x. The experimental data are taken from Torres and Stradling [44]

PROPERTIES OF SEMICONDUCTOR ALLOYS

meΓ/m0

meΓ/m0

256

0.16 0.14 (a) GaxIn1-xAs 0.12 x = 0.22 ( ) 0.34 0.10 0.47 0.08 0.06 0.04 18 10 1019 0.18 0.16 (b) InP xAs1-x 0.14 x = 0.29 0.12 0.48 ( ) 0.69 0.10 0.08 0.06 0.04 18 10 1019 n (cm-3)

1020

1020

Figure 7.28 Free-electron concentration dependence of mGe in (a) GaxIn1xAs and (b) InPxAs1x. The experimental data are taken from Metzger et al. [75]. The solid lines show the least-squares fits given by (a) ln(mGe /m0) ¼ (2.24 1020)n 2.89 (x ¼ 0.22) and (b) ln(mGe /m0) ¼ (2.04 1020)n 2.95 (x ¼ 0.48) with n in cm3, respectively

The highest VBs and lowest CB of III–Vand II–VI semiconductors are nonparabolic. Since the band nonparabolicity becomes significant as the Fermi level moves deep in the band, the electron effective mass in semiconductors increases with doping level for carrier concentrations larger than 1018 cm3. The dependence of the electron effective mass mGe on electron concentration in GaxIn1xAs and InPxAs1x has been reported by Metzger et al. [75]. Their results are reproduced in Figure 7.28. The electron effective masses increase abruptly as a function of free-electron density and converge at n 5 1019 cm3. They concluded that the Kanes band model offers an accurate description of CB nonparabolicity. An increase in m*e with increasing free-electron density has also been observed in dilute-nitride GaxIn1xNyAs1y [74].

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] T. Hofmann, T. Chavdarov, V. Darakchieva, H. Lu, W. J. Schaff, and M. Schubert, Phys. Status Solidi C 3, 1854 (2006). [3] D. Fritsch, H. Schmidt, and M. Grundmann, Phys. Rev. B 69, 165204 (2004). [4] D. Bimberg, M. Altarelli, and N. O. Lipari, Solid State Commun. 40, 437 (1981). [5] D. Fink and R. Braunstein, Phys. Status Solidi B 73, 361 (1976). [6] C. W. Liu and V. Venkataraman, Mater. Chem. Phys. 49, 29 (1997). [7] J. F. N€utzel, C. M. Engelhardt, and G. Abstreiter, in Properties of Strained and Relaxed Silicon Germanium, EMIS Datareviews Series No. 12 (edited by E. Kasper), INSPEC, London, 1995, p. 103. [8] P. Emanuelsson, M. Drechsler, D. M. Hofmann, and B. K. Meyer, Appl. Phys. Lett. 64, 2849 (1994). [9] S. Adachi, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, pp. 58–72.

ENERGY-BAND STRUCTURE: EFFECTIVE MASSES

257

[10] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [11] J. C. Hensel and K. Suzuki, Phys. Rev. B 9, 4219 (1974). [12] E. E. Matyas and A. G. Karoza, Phys. Status Solidi B 111, K45 (1982). [13] M. G. Wright, A. Kanaah, B. C. Cavenett, G. R. Johnson, and S. T. Davey, Semicond. Sci. Technol. 4, 590 (1989). [14] L. A. Cury, J. Beerens, and J. P. Praseuth, Appl. Phys. Lett. 63, 1804 (1993). [15] Y. F. Chen, Y. T. Dai, J. C. Fan, T. L. Lee, and H. H. Lin, Appl. Phys. Lett. 67, 1256 (1995). [16] M. B. Thomas and J. C. Woolley, Can. J. Phys. 49, 2052 (1971). [17] H. Fetterman, J. Waldman, and C. M. Wolfe, Solid State Commun. 11, 375 (1972). [18] C. K. Sarkar, R. J. Nicholas, J. C. Portal, M. Razeghi, J. Chevrier, and J. Massies, J. Phys. C: Solid State Phys. 18, 2667 (1985). [19] Y. T. Dai, J. L. Shen, Y. F. Chen, S. Z. Chang, and S. C. Lee, Chin. J. Phys. 36, 20 (1998). [20] J. L. Shen, Y. D. Dai, Y. F. Chen, S. Z. Chang, and S. C. Lee, Phys. Rev. B 51, 17648 (1995). [21] K. Alavi, R. L. Aggarwal, and S. H. Groves, Phys. Rev. B 21, 1311 (1980). [22] R. J. Warburton, R. W. Martin, R. J. Nicholas, L. K. Howard, and M. T. Emeny, Semicond. Sci. Technol. 6, 359 (1991). [23] N. J. Traynor, R. J. Warburton, M. J. Snelling, and R. T. Harley, Phys. Rev. B 55, 15701 (1997). [24] M. J. Aubin, M. B. Thomas, E. H. van Tongerloo, and J. C. Woolley, Can. J. Phys. 47, 631 (1969). [25] A. P. Roth and E. Fortin, Can. J. Phys. 56, 1468 (1978). [26] H. P. Xin and C. W. Tu, Appl. Phys. Lett. 77, 2180 (2000). [27] P. N. Hai, W. M. Chen, I. A. Buyanova, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 77, 1843 (2000). [28] J. Wu, W. Shan, W. Walukiewicz, K. M. Yu, J. W. Ager III, E. E. Haller, H. P. Xin, and C. W. Tu, Phys. Rev. B 64, 085320 (2001). [29] Y. J. Wang, X. Wei, Y. Zhang, A. Mascarenhas, H. P. Xin, Y. G. Hong, and C. W. Tu, Appl. Phys. Lett. 82, 4453 (2003). [30] F. Masia, A. Polimeni, G. B. H. von H€ogersthal, M. Bissiri, P. J. Klar, and W. Stolz, Appl. Phys. Lett. 82, 4474 (2003). [31] F. Masia, G. Pettinari, A. Polimeni, M. Felici, A. Miriametro, M. Capizzi, A. Lindsay, S. B. Healy, E. P. OReilly, A. Cristofoli, G. Bais, M. Piccin, S. Rubini, F. Martelli, A. Faranciosi, P. J. Klar, K. Volz, and W. Stolz, Phys. Rev. B 73, 073201 (2006). [32] Y. Zhang and A. Mascarenhas, Phys. Rev. B 61, 7479 (2000). [33] D. L. Young, J. F. Geisz, and T. J. Coutts, Appl. Phys. Lett. 82, 1236 (2003). [34] See, for example, M. Henini, Dilute Nitride Semiconductors, Elsevier, Amsterdam, 2005. [35] W. K. Hung, K. S. Cho, M. Y. Chern, Y. F. Chen, D. K. Shih, H. H. Lin, C. C. Lu, and T. R. Yang, Appl. Phys. Lett. 80, 796 (2002). [36] D. R. Hang, C. F. Huang, W. K. Hung, Y. H. Chang, J. C. Chen, H. C. Yang, Y. F. Chen, D. K. Shih, T. Y. Chu, and H. H. Lin, Semicond. Sci. Technol. 17, 999 (2002). [37] D. -K. Shih, H. -H. Lin, L. -W. Sung, T. -Y. Chu, and T. -R. Yang, Jpn. J. Appl. Phys. 42, 375 (2003). [38] B. N. Murdin, A. R. Adams, P. Murzyn, C. R. Pidgeon, I. V. Bradley, J. -P. R. Wells, Y. H. Matsuda, N. Miura, T. Burke, and A. D. Johnson, Appl. Phys. Lett. 81, 256 (2002). [39] C. Wetzel, B. K. Meyer, and P. Omling, Phys. Rev. B 47, 15588 (1993). [40] A. Filion and E. Fortin, Can. J. Phys. 52, 743 (1974). [41] R. J. Nicholas, R. A. Stradling, and J. C. Ramage, J. Phys. C: Solid State Phys. 12, 1641 (1979). [42] R. J. Nicholas, R. A. Stradling, J. C. Portal, and S. Askenazy, J. Phys. C: Solid State Phys. 12, 1653 (1979). . Rut, Sov. Phys. Semicond. 16, 596 (1982). [43] V. V. Kruzhaev, G. M. Minkov, and O. E [44] C. M. S. Torres and R. A. Stradling, Semicond. Sci. Technol. 2, 323 (1987). [45] T. W. Kim, D. C. Choo, D. U. Lee, M. Jung, and S. O. Kang, J. Phys. Chem. Solids 63, 875 (2002). [46] M. B. Thomas and J. C. Woolley, Can. J. Phys. 49, 2056 (1971).

258

PROPERTIES OF SEMICONDUCTOR ALLOYS

[47] S. N. Smith, C. C. Phillips, R. H. Thomas, R. A. Stradling, I. T. Ferguson, A. G. Norman, B. N. Murdin, and C. R. Pidgeon, Semicond. Sci. Technol. 7, 900 (1992). [48] Z. Pan, L. H. Li, Y. W. Lin, B. Q. Sun, and D. S. Jiang, Appl. Phys. Lett. 78, 2217 (2001). [49] J. B. Herouz, X. Yang, and W. I. Wang, J. Appl. Phys. 92, 4361 (2002). [50] M. Hetterich, M. D. Dawson, A. Y. Egorov, D. Bernkiau, and H. Riechert, Appl. Phys. Lett. 76, 1030 (2000). [51] C. Skierbiszewski, P. Perlin, P. Wisniewski, W. Knap, T. Suski, W. Walukiewicz, W. Shan, K. M. Yu, J. W. Ager, E. E. Haller, J. F. Geisz, and J. M. Olson, Appl. Phys. Lett. 76, 2409 (2000). [52] J. -Y. Duboz, J. A. Gupta, M. Byloss, G. C. Aers, H. C. Liu, and Z. R. Wasilewski, Appl. Phys. Lett. 81, 1836 (2002). [53] C. Skierbiszewski and J. Łusakowski, J. Phys.: Condens. Matter 16, S3319 (2004). [54] M. H. Gass, A. J. Papworth, T. B. Joyce, T. J. Bullough, and P. R. Chalker, Appl. Phys. Lett. 84, 1453 (2004). [55] A. Polimeni, F. Masia, A. Vinattieri, G. B. H. von H€ ogersthal, and M. Capizzi, Appl. Phys. Lett. 84, 2295 (2004). [56] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992. [57] D. Olego, T. Y. Chang, E. Silberg, E. A. Caridi, and A. Pinczuk, Appl. Phys. Lett. 41, 476 (1982). [58] R. F. Kopf, H. P. Wei, A. P. Perley, and G. Livescu, Appl. Phys. Lett. 60, 2386 (1992). [59] T. I. Voronina, T. S. Lagunova, K. D. Moiseev, M. A. Sipovskaya, I. N. Timchenko, and Y. P. Yakovlev, Semicond. 27, 978 (1993). [60] J. G. Lu, S. Fujita, T. Kawaharamura, H. Nishinaka, Y. Kamada, and T. Ohshima, Appl. Phys. Lett. 89, 262107 (2006). [61] Y. Imanaka and N. Miura, Physica B 249–251, 932 (1998). [62] I. Lo, S. J. Chen, L. -W. Tu, W. C. Mitchel, R. C. Tu, and Y. K. Su, Phys. Rev. B 60, R11281 (1999). [63] H. K. Ng, Y. A. Leem, R. Knobel, I. P. Smorchkova, A. A. Sirenko, and N. Samarth, Appl. Phys. Lett. 75, 3662 (1999). [64] H. Shao, S. Scholl, H. Sch€afer, J. Gersch€utz, B. Jobst, D. Hommel, and G. Landwehr, Solid State Commun. 100, 739 (1996). [65] A. D. Shneider and D. I. Tsiutsiura, Phys. Status Solidi A 5, K39. (1971). [66] R. S. Kim and S. Narita, Phys. Status Solidi B 73, 741 (1976). [67] J. P. Laurenti, J. Camassel, A. Bouhemadou, B. Toulouse, R. Legros, and A. Lusson, J. Appl. Phys. 67, 6454 (1990). [68] J. Chu, Z. Mi, and D. Tang, Infrared Phys. 32, 195 (1991). [69] Y. -G. Sha, C. -H. Su, and S. L. Lehoczky, J. Appl. Phys. 81, 2245 (1997). [70] M. S. Brodin, M. V. Kurik, and S. P. Yurtsenyuk, Sov. Phys. Solid State 7, 2516 (1966). [71] D. Gauthier, L. Dmowski, J. C. Portal, D. Leadley, M. A. Hopkins, M. A. Brummell, R. J. Nicholas, M. Razeghi, and P. Maurel, Superlatt. Microstruct. 4, 201 (1988). [72] S. Charlebois, J. Beerens, C. J. Miner, and N. Puetz, Phys. Rev. B 54, 13456 (1996). [73] C. Skierbiszewski, P. Erlin, P. Wisniewski, T. Suski, J. F. Geisz, K. Hingerl, W. Jantsch, D. E. Mars, and W. Walukiewicz, Phys. Rev. B 65, 035207 (2001). [74] C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002). [75] W. K. Metzger, M. W. Wanlass, L. M. Gedvilas, J. C. Verley, J. J. Carapella, and R. K. Ahrenkiel, J. Appl. Phys. 92, 3524 (2002).

8 Deformation Potentials 8.1 INTRAVALLEY DEFORMATION POTENTIAL: G POINT 8.1.1 Group-IV Semiconductor Alloy A review of the various DPs is given in Adachi [1]. The G-valley DPs (aGc ¼ E1G and Di) in the CB of some non-alloyed ANB8N tetrahedral semiconductors are summarized in Tables 8.1 and 8.2. Tables 8.3 and 8.4 also summarize the G-point DPs a, b, d and Ci in the VB for some cubic and wurtzite semiconductors, respectively. Table 8.1 Intravalley deformation potential, aGc ¼ E1G , for electrons at the G point of some cubic group-IV, III–V and II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

aGc (eV)

System

Material

aGc (eV)

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

30.7a,b 15.3a,b 8.24a,b 13.7a,b 7.50b

II–VI

ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb)

4.09b 4.17b 5.83b 27.1b 11.0b 3.96b

III–V

BN (zb) BP (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb) InSb (zb)

36.5b 13.3b 11.7b 5.54b 5.64b 6.97b 21.3b 7.14b 11.0 9 11.4 10.2 15

HgTe (zb)

4.60b

a b

G20 -conduction band Calculated

No experimental determinations of the intravalley DPs in the G valley for group-IV semiconductor alloys appear to be available. The interpolated DPs for SixGe1x obtained by Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

260

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 8.2 Intravalley deformation potentials, D1 and D2, for electrons at the G point of some wurtzite III–V semiconductors System

Material

D1 (eV)

D2 (eV)

III–V

AlN GaN

10.23a 9.47a

9.65a 7.17a

a

Calculated

Table 8.3 Deformation potentials, a, b and d, for holes at the G point of some cubic group-IV, III–Vand II–VI semiconductors. d ¼ diamond; zb ¼ zinc-blende System

Material

a (eV)

b (eV)

d (eV)

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

36.1a 5 5.2 3.3a 4.30a

11.1a 2.3 2.4 2.3 2.20a

5.3 4.8 4.1 6.26a

III–V

BN (zb) BP (zb) BAs (zb) AlN (zb) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaP (zb) GaAs (zb) GaSb (zb) InP (zb) InAs (zb) InSb (zb)

7.3a 4.2a

3.41a 4.9a 4.5a 1.7a 1.5a 2.3a 1.35 2.09a 1.7 1.85 2.4 1.7 1.8 2.0

II–VI

a

Calculated

MgSe (zb) ZnS (zb) ZnSe (zb) ZnTe (zb) CdS (zb) CdSe (zb) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

5.9a 3.15a 2.6a 1.38a 13.33a 1.70a 0.85 0.79a 0.6 1.00a 0.36a 1.0a 2.31a 1.65a 0.79a 0.92a 8.9a 0.55a 0.13a

1.27a 1.1 1.8 1.4 4.7 0.8 1.0 1.24a 1.16a 1.5

3.75a 4.4a 4.3 1.75a 4.4 5.1 5.4 4.3 3.6 5.4 4.4 5.0 4.4 4.4 8.0

DEFORMATION POTENTIALS

261

Table 8.4 Deformation potential Ci for holes at the G point of some wurtzite III–V and II–VI semiconductors (in eV) D1–C1

System

Material

C1

III–V

AlN GaN InN

12.9a 41.4

II–VI

ZnO CdS CdSe

a

3.1 4.05a

C2 8.4a 33.3

3.90 1.36 0.76

D2–C2

C3

C4

C5

C6

11.2 6.67a

4.5a 8.2 4.92a

2.2a 4.1 1.79a

2.6a 4.7

4.1a

4.13 2.28 3.7

1.15 1.54 4.0

1.22 2.34 2.2

1.53 1.20 1.2

2.88 3.0

Calculated

introducing the Si and Ge values in Tables 8.1 and 8.3 into Equation (A.16) are therefore plotted in Figure 8.1. The solid circles in Figure 8.1(b) show the theoretical b values obtained by Schmid et al. [2]. Rieger and Vogl [3] also reported the theoretical b versus x data for SixGe1x, which vary from 2.1 (x ¼ 0) to 2.3 eV (x ¼ 1.0). 0

0 (a)

(b) -1

SixGe1-x a, b, d (eV)

acΓ (eV)

-4 -8 -12

-2 b

-3 -4

-16 -20

d

-5 0

0.2 0.4 0.6 0.8 1.0 x

-6

0

a

0.2 0.4 0.6 0.8 1.0 x

Figure 8.1 (a) CB DP aGc and (b) VB DPs a, b and d for SixGe1x. The solid lines are obtained by introducing the endpoint elemental data into Equation (A.16). The solid circles in (b) show the theoretical b values calculated by Schmid et al. [2]

The E0-gap DP aG0 for some non-alloyed group-IV, III–V and II–VI semiconductors is listed in Table 8.5. Schmid et al. [2] reported a theoretical aG0 value of 11.5 eV for Si0.5Ge0.5. No experimental data are available for group-IV semiconductor alloys.

8.1.2 III–V Semiconductor Ternary Alloy (a) AlGaN The E0-gap DP aG0 can be simply obtained if the pressure coefficient dE0/dp and bulk modulus Bu are available [1]. The pressure coefficient for w-AlxGa1xN has been measured by

262

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 8.5 Hydrostatic deformation potential aG0 for the E0 gap of some cubic and hexagonal semiconductors. d ¼ diamond; zb ¼ zinc-blende; w ¼ wurtzite System

Material

aG0 (eV)

System

Material

aG0 (eV)

IV

Diamond (d) Si (d) Ge (d) a-Sn (d) 3C-SiC (zb)

27a,b 11.84a,b 9.8a 7.04a,b 11.5b

II–VI

MgSe (zb) ZnO (w) ZnS (zb) ZnS (w)

4.2b 3.51 (A) 3.59 (B) 3.81 (C) 5.2 4.7b

BP (zb) AlN (zb) AlN (w) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

17.5b 9.5b 10.3b 9.52b 8.93b 5.9 9.0b 8.8 9.3 8.8 8.3 4.2b 6.0 6.3 7.0

ZnSe (zb) ZnTe (zb) CdS (zb) CdS (w) CdSe (zb) CdSe (w) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

5.1 5.3 0.43b 2.9 0.80b 2.3 2.9 2.16b 2.15b 3.69

III–V

a v b

G250 –Gc20 gap Calculated or estimated

Shan et al. [4]. The x-dependent Bu value for this alloy can be easily obtained by introducing the AlN and GaN values in Table 3.22 of Adachi [1] into the linear interpolation expression. The results obtained are shown in Figure 8.2(a). (b) GaInN The pressure coefficient dE0/dp for w-GaxIn1xN has been measured by Li et al. [5] and also discussed both theoretically and experimentally by Franssen et al. [6]. Figure 8.2(b) shows the aG0 versus x plots for w-GaxIn1xN obtained using the same procedure as in Figure 8.2(a). (c) AlInP Figure 8.3(a) shows the shear DPs b and d versus x for AlxIn1xP. Ishitani et al. [7] determined the shear DP b ¼ 1.67 0.26 eV for AlxIn1xP (0.43 x 0.62) grown on GaAs(100) by MOCVD using PR. This value is plotted in Figure 8.3(a) by the solid circle. The linear interpolation scheme is found to give satisfactory agreement with the experimental data.

DEFORMATION POTENTIALS 0

263

0 (a) w-AlxGa1-xN -4 a0Γ (eV)

a0Γ (eV)

-4

-8

-12

-8

-12 (b) w-GaxIn1-xN

-16

0

0.2 0.4 0.6 0.8 1.0 x

-16

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.2 aG0 for (a) w-AlxGa1xN and (b) w-GaxIn1xN. The solid circles are deduced from the experimental dE0/dp data of (a) Shan et al. [4] and (b) Li et al. [5]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

(d) GaInP The shear DPs b and d versus x for GaxIn1xP are shown plot in Figure 8.3(b). The solid circle represents the experimental data d ¼ 4.0 0.2 eV taken from Bolkhovityanov et al. [8]. This data deviates slightly from the linear interpolation result. 0

0 (a) AlxIn1-xP

-0.8

b

b, d (eV)

-1.6

(b) GaxIn1-xP

-0.8

-2.4

-2.4

-3.2

-3.2

-4.0

b

-1.6

-4.0

d

d

-4.8

0

0.2 0.4 0.6 0.8 1.0 x

-4.8

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.3 Shear DPs b and d for (a) AlxIn1xP and (b) GaxIn1xP. The experimental data in (a) are taken from Ishitani et al. [7] and in (b) from Bolkhovityanov et al. [8]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

(e) AlGaAs Figure 8.4(a) shows the DPs a, b and d for AlxGa1xAs. The experimental data are taken from Qiang et al. [9,10]. The solid lines (a and b) show the linear interpolation results obtained by introducing the GaAs (x ¼ 0) and AlAs (x ¼ 1.0) values in Table 8.3 into Equation (A.4).

264

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 8.4(b) shows the E0-gap DP aG0 for AlxGa1xAs. The solid circles are obtained from the experimental data for dE0/dp (Figure 6.21(b)) using the same procedure as in Figure 8.2(a). The aG0 value is found to be 8.9 eV, i.e. independent of x. 0

0

-1

a

-3

-2

AlxGa1-xAs

b

-3

a0Γ (eV)

a, b, d (eV)

(b)

(a)

-6

-4 -5

-9

d

-6 -7

0

0.2 0.4 0.6 0.8 1.0 x

-12

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.4 (a) DPs a, b and d and (b) aG0 for AlxGa1xAs. The experimental data in (a) are taken from Qiang et al. [9,10]. The aG0 values in (b) are deduced from the experimental dE0/dp data in Figure 6.21(b). The solid lines for a and b in (a) are obtained by introducing the endpoint binary data into Equation (A.4)

(f) AlInAs The DPs a, b and d for AlxIn1xAs are shown in Figure 8.5(a). The experimental data are taken from Yeh et al. [11] (open circle) and Pavesi et al. [12] (solid circle). The E0-gap DP values aG0 measured by Pavesi et al. [12] (solid circle) and Ferguson et al. [13] (solid triangle) are also shown in Figure 8.5(b), together with the endpoint binary data (open squares).

2.0

0

(a)

1.0

AlxIn1-xAs

-4 a

-1.0 -2.0

b

-3.0

a0Γ (eV)

0 a, b, d (eV)

(b)

-2

-6 -8

-10 d

-4.0

0

0.2 0.4 0.6 0.8 1.0 x

-12

0

0.2 0.4 0.6 0.8 1.0 x

Figure 8.5 (a) DPs a, b and d and (b) aG0 for AlxIn1xAs. The solid lines in (a) and (b) are obtained by introducing the endpoint binary data into Equation (A.4). The open circle in (a) represents the experimental data of Yeh et al. [11], while the solid circles in (a) and (b) are taken from Pavesi et al. [12]. The solid triangle in (b) also shows the experimental data of Ferguson et al. [13]

DEFORMATION POTENTIALS

265

(g) GaInAs Figure 8.6 shows the E0-gap DP aG0 versus x for GaxIn1xAs. The experimental data obtained by People et al. [14] for x ¼ 0.47 is shown in Figure 8.5(b) by the solid circle, together with the endpoint binary data (open squares). These data give the following quadratic least-squares fit (in eV) aG0 ðxÞ ¼ 6:33:8x þ 1:3x2 ð8:1Þ Wilkinson et al. [15] reported the x-dependent aG0 value for GaxIn1xAs to be aG0 ¼ 7.993.76x eV. However, the InAs value, aG0 ¼ 7.99 eV, obtained from this expression predicts a considerably large pressure coefficient dE0/dp 1.4 101 eV/GPa. A pressure coefficient as large as this has never been reported in the literature. (Only values in the range of dE0/dp ¼ (9.56–11.4) 102 eV/GPa have been reported in the literature [16]). 0

a0Γ (eV)

-2

GaxIn1-xAs

-4 -6 -8 -10 -12

0

0.2

0.4

x

0.6

0.8

1.0

Figure 8.6 aG0 for GaxIn1xAs. The solid circle shows the experimental data of People et al. [14]. The solid line represents the calculated result using Equation (8.1)

(h) GaNAs The shear DP b for dilute-nitride GaNxAs1x has been determined using ER [17] and PR [18]. The data obtained by Zhang et al. [17] (solid circles) and Ya et al. [18] (open circles) are shown in Figure 8.7. These data show a surprising bowing in a small range of alloy compositions and exhibit a minimum at x 1.7 at%. The quadratic least-squares fit of these data can be written as 0 GaNx As1-x

b (eV)

-1 -2 -3 -4

0

1

2

3 x (at%)

4

5

Figure 8.7 Shear DP b for dilute-nitride GaNxAs1x. The experimental data are obtained from Zhang et al. [17] (solid circles) and Ya et al. [18] (open circles). The solid line shows the calculated result using Equation (8.2)

266

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b in eV, x in at%) bðxÞ ¼ 1:850:99x þ 0:29x2

ð8:2Þ

The results contradict the currently held view that the CB is greatly altered but the VB is only weakly perturbed by dilute N doping of III–V semiconductors. (i) GaPAs

a, b, d (eV)

The DPs a, b and d for GaPxAs1x are shown in Figure 8.8. The solid circles represent the experimental b values obtained by Gonzalez et al. [19]. It can be seen that the linear interpolation scheme traces the experimental DP data very well. 2 1 0 -1 -2 -3 -4 -5 -6

a

b

GaPxAs1-x

0

0.2

d

0.4

0.6

0.8

1.0

x

Figure 8.8 DPs a, b and d for GaPxAs1x. The solid circles show the experimental data reported by Gonzalez et al. [19]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

8.1.3 III–V Semiconductor Quaternary Alloy There has been no detailed experimental data relating to a, b or d for any III–V quaternary. Therefore, the linearly interpolated a, b and d values for GaxIn1xPyAs1y/InP using Equation (A.6) are plotted in Figure 8.9(a). The DPs a and d show upward bowing against y, while b varies almost linearly with y. Figure 8.9(b) shows the E0-gap DP aG0 versus y for GaxIn1xPyAs1y/InP. The solid circles represent the experimental data obtained from the pressure coefficients dE0/dp (Figure 6.46(b)) using the same procedure as in Figure 8.2(a). The solid line represents the linearly interpolated aG0 values obtained by introducing the binary data into Equation (A.6). The experimental aG0 values for GaxIn1xPyAs1y/InP are found to be well interpreted by the linear interpolation expression (in eV) aG0 ðxÞ ¼ 7:6 þ 1:6x ð8:3Þ

8.1.4 II–VI Semiconductor Alloy The shear DPs b and d versus x for ZnxCd1xTe are shown in Figure 8.10. The solid circle shows the experimental value b ¼ 1.07 0.06 eV for x ¼ 0.605 determined by Pelhos et al. [20].

DEFORMATION POTENTIALS 1

-3

0

Gax In1-x Py As1-y /InP

a

-6

b

-2

a0Γ (eV)

a, b, d (eV)

-1

-3

-9

d

-4 -5 -6 0

267

(a)

(b)

-12 0

0.2 0.4 0.6 0.8 1.0 y

0.2 0.4 0.6 0.8 1.0 y

Figure 8.9 (a) DPs a, b and d and (b) aG0 for GaxIn1xPyAs1y/InP. The solid circles in (b) are deduced from the experimental dE0/dp data in Figure 6.46(b). The solid lines in (a) and (b) are obtained by introducing the binary data into Equation (A.6) 0

b, d (eV)

-1

b

-2 ZnxCd1-xTe

-3 -4

d

-5 -6

0

0.2

0.4

0.6

0.8

1.0

x

Figure 8.10 Shear DPs b and d for ZnxCd1xTe. The solid circle shows the experimental data reported by Pelhos et al. [20]. The solid lines are obtained by introducing the endpoint binary data into Equation (A.4)

The pressure coefficient dE0/dp has been measured on some II–VI semiconductor alloys, such as w-MgxZn1xO [21], w-ZnxCd1xS [22], c-ZnOxSe1x [23], ZnSxSe1x [24], ZnSxTe1x [25] and ZnSexTe1x [26]. By introducing these pressure coefficients and interpolated Bu values (Tables 3.17 and 3.22 in Adachi [1]) into Equation (8.14) of Adachi [1], aG0 for such II–VI semiconductor alloys can be obtained.

8.2 INTRAVALLEY DEFORMATION POTENTIAL: HIGH-SYMMETRY POINTS 8.2.1 Group-IV Semiconductor Alloy The L-valley DPs for some non-alloyed ANB8N tetrahedral semiconductors are summarized in Tables 8.6–8.8. Table 8.9 also summarizes the X (D)-valley DPs for some non-alloyed groupIV and III–V semiconductors.

268

PROPERTIES OF SEMICONDUCTOR ALLOYS

Table 8.6 Hydrostatic E1 and shear deformation potentials E2 for electrons at the L point of some cubic group-IV and III–V semiconductors System

Material

IV

Si Ge

a b

E1 (eV)

E2 (eV)

3.1a 3.8

18.0a 15.9

System

Material

III–V

c-BN c-AlN AlAs b-GaN GaAs GaSb

E1 (eV)

E2 (eV) 27.9a 25.5a

4.2b

27.5a 14.5 17.5

2 3.2

Calculated Estimated

Table 8.7 Deformation potentials, D53 and D33 , for holes at the L point of some cubic group-IV, III–V and II–VI semiconductors determined experimentally System

Material

IV

Si Ge

III–V

GaAs InP

D53 (eV) 4.3 3.7 6.4 12.9

D33 (eV)

System

Material

D53 (eV)

D33 (eV)

4.6 5.6 (E1) 6.2 (E1 þ D1)

II–VI

ZnSe ZnTe

27 15

17 29

5.4 4.1

pﬃﬃﬃ Table 8.8 Hydrostatic D11 ¼ 3aL1 and interband deformation potentials D51 for the E1 and E1 þ D1 gaps of some cubic group-IV, III–V and II–VI semiconductors determined experimentally System

Material

IV

Si Ge

III–V

GaAs GaSb InP InSb

II–VI

ZnSe ZnTe

D11 (eV) 9.0 8.7 8.3 12.3 (E1) 17.7 (E1 þ D1) 9.2 7.4 (E1) 8.5 (E1 þ D1) 5.8 5.5

D51 (eV) 9 12.2 12.0 7.4 (E1) 20.4 7.4 (E1) 6.5 (E1 þ D1) 30 40

DEFORMATION POTENTIALS

269

Table 8.9 Hydrostatic E1 and shear deformation potentials E2 for electrons at the X point of some cubic group-IV and III–V semiconductors System

Material

IV

Si Ge

a b

E1 (eV)

E2 (eV)

4.2 5.75a

9.6 9.75a

System

Material

III–V

c-BN c-AlN AlP AlAs AlSb b-GaN GaP GaAs GaSb InP InAs InSb

E1 (eV) 5.5 1.81a 1.20 a

6.8a 2.7 1.05b 1.99a 1.85a 1.59a 1.56a

E2 (eV) 17.9a 6.6a 6.75a 6.9 5.4 7.1a 6.3 6.5 6.46a 3.3a 3.7a 4.53a

Calculated Estimated

Although there have been several theoretical studies on the DPs at the high-symmetry points of SixGe1x [2,3], no experimental determinations appear to be available for any group-IV semiconductor alloy. Figure 8.11 shows the linearly interpolated L- and X-valley DPs E1(L) and E1(X) at the CB, respectively, obtained by introducing the Si and Ge values in Tables 8.6 and 8.9 into Equation (A.16). The crossing of the lowest-lying CB states from the L point to the X (D) point can be seen at x 0.15 (Figure 6.8). Thus, the nature of the conduction electron in SixGe1x changes from ‘Ge-like’ to ‘Si-like’ at x 0.15. 8 L-X (Δ) crossing

E1(L) (eV)

-1.6

SixGe1-x

6

-2.4 4 -3.2 2

-4.0 -4.8

E1(X) (eV)

-0.8

(Ge-like)

0

0.2

0.4

x

0.6

0.8

0 1.0

Figure 8.11 L- and X-valley DPs E1(L) and E1(X) at the CB for SixGe1x. The solid lines are obtained by introducing the endpoint elemental data into Equation (A.16). The dashed line indicates the L–X (D) crossing composition xc 0.15

8.2.2 III–V Semiconductor Alloy Figure 8.12 shows the X-valley DP E1 in the CB versus x for AlxGa1xAs. The experimental data are taken from Adachi [27]. These data provide the following x variation: E1 ¼ 1.05 þ 0.15x eV. The solid line in Figure 8.12 shows the result of this variation.

270

PROPERTIES OF SEMICONDUCTOR ALLOYS

E1(X) (eV)

2.0 AlxGa1-x As

1.5 1.0 0.5 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 8.12 X-valley DP E1 in the CB for AlxGa1xAs. The experimental data are taken from Adachi [27]. The solid line shows the linearly interpolated result using the endpoint binary data

Figure 8.13 plots the L-valley DP D33 in the VB for GaPxAs1x. The solid circles show the experimental data obtained by Gonzalez et al. [19] determined using ER. The solid line represents the calculated result of D33 ¼ 5.4 þ 5.0x eV. This expression predicts a GaP (x ¼ 1.0) value of 0.4 eV. The experimental D53 and D33 values reported for non-alloyed ANB8N tetrahedral semiconductors are limited to Si, Ge, GaAs, InP, ZnSe and ZnTe (Table 8.7, see also Adachi [16,28,29]). 0

D33 (eV)

-1 GaPx As1-x

-2 -3 -4 -5 -6 0

0.2

0.4

x

0.6

0.8

1.0

Figure 8.13 L-valley DP D33 in the VB for GaPxAs1x. The solid circles show the experimental data of Gonzalez et al. [19]. The solid line represents the calculated result of D33 ¼ 5.4 þ 5.0x eV

8.2.3 II–VI Semiconductor Alloy No detailed data are available for II–VI semiconductor alloys.

8.3 INTERVALLEY DEFORMATION POTENTIAL 8.3.1 Group-IV Semiconductor Alloy The intervalley DPs for some non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Tables 8.10 and 8.11. Unfortunately, no detailed data are available for group-IV semiconductor alloys.

DEFORMATION POTENTIALS

271

Table 8.10 Intervalley deformation potential Dij for electrons in some cubic group-IV, III–V and II–VI semiconductors (in eV/A) System

Material

IV

Diamond Si Ge

2.0

III–V

AlP AlAs AlSb GaP GaAs GaSb InP InAs InSb

5.0 1.6–2.3 2.3–3.4 0.7–1.1 1.5–9.5 2.7–2.8 1.3–2.7 1.0–2.0 1.1–4.3

5.0 3.1 1.3–4.9 0.8–1.1 5.2–15 2.5–4.5 1.6 2.0–2.2 3.3–4.9

II–VI

b-ZnS ZnSe ZnTe CdTe

2.18–4.13 2.17–2.71 3.19–3.31 1.68–1.76

1.10–1.89 0.72–1.37 1.17–1.43 0.40–1.23

a

DGL

DGXa

DLL

10.0

2.63 0.2–3.0

DXX 8.0 0.15–4.0 0.79–9.5

0.3–1.0 1.6 0.5–0.6 0.6 5 0.6–1.2 0.3–0.9 1.1 0.3–0.6

8.1 4.7 9.5 3.0 10 6.0 3.6 2.5 6.8

DLX 4.0 4.1 0.4–1.7 0.8–3.7 0.4–1.6 2.75–3.1 1.0–2.2 0.7–3.3 0.6–1.9 0.2–2.9

DGX(1) and DGX(3)

Table 8.11 Intervalley deformation potential Dij for electrons in some hexagonal III–V semiconductors

Dij (eV/A)

Material

w-AlN a-GaN InN

Equivalent valley

Nonequivalent valley

10 5–10 10

10 10 10

8.3.2 III–V Semiconductor Alloy Parker et al. [30] observed field-assisted emission from a heterostructure with a GaAs–Al0.25 Ga0.75As emitter layer and derived information on hot-electron energy distributions at the low electron density limit. From computer-modeled analysis, they deduced the intervalley coupling constants Dij for Al0.25Ga0.75As. These results are shown in Figure 8.14 together with those for AlAs and GaAs (Table 8.10).

272

PROPERTIES OF SEMICONDUCTOR ALLOYS 15

15 AlxGa1-x As

Dij (eV/Å)

10

10

DΓL

5

5

0 15

0 15

10

10

DΓX

5

5

0 15

0

10

DXX

DLX

0

0.2

0.4

x

0.6

0.8

1.0

DLL

5 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 8.14 Intervalley coupling constants Dij for AlxGa1xAs. The solid circles show the Al0.25Ga0.75As values deduced from field-assisted emission data reported by Parker et al. [30]

8.3.3 II–VI Semiconductor Alloy No detailed data are available for II–VI semiconductor alloys.

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] U. Schmid, N.E. Christensen, and M. Cardona, Solid State Commun. 75, 39 (1990). [3] M.M. Rieger and P. Vogl, Phys. Rev. B 48, 14276 (1993). [4] W. Shan, J.W. Ager III, K.M. Yu, W. Walukiewicz, E.E. Haller, M.C. Martin, W.R. McKinney, and W. Yang, J. Appl. Phys. 85, 8505 (1999). [5] S.X. Li, J. Wu, W. Walukiewicz, W. Shan, E.E. Haller, H. Lu, W.J. Schaff, Y. Saito, and Y. Nanishi, Phys. Status Solidi B 241, 3107 (2004). [6] G. Franssen, I. Gorczyca, T. Suski, A. Kami nska, J. Pereiro, E. Mu~ noz, E. Iliopoulos, A. Georgakilas, S.B. Che, Y. Ishitani, A. Yoshikawa, N.E. Christensen, and A. Svane, J. Appl. Phys. 103, 033514 (2008). [7] Y. Ishitani, H. Hamada, S. Minagawa, H. Yaguchi, and Y. Shiraki, Jpn. J. Appl. Phys. 36, 6607 (1997). [8] Y.B. Bolkhovityanov, A.S. Jaroshevich, M.A. Revenko, H.E. Scheibler, and A.S. Terekhov, Semicond. Sc. Technol. 11, 1847 (1996). [9] H. Qiang, F.H. Pollak, and G. Hickman, Solid State Commun. 76, 1087 (1990). [10] H. Qiang, F.H. Pollak, and R.N. Sacks, Solid State Commun. 84, 51 (1992). [11] C.N. Yeh, L.E. McNeil, R.E. Nahory, and R. Bhat, Phys. Rev. B 52, 14682 (1995). [12] L. Pavesi, R. Houdre, and P. Giannozzi, J. Appl. Phys. 78, 470 (1995). [13] I.T. Ferguson, T.P. Beales, T.S. Cheng, C.M. Sotomayor-Torres, and E.G. Scott, Semicond. Sci. Technol. 4, 243 (1989). [14] R. People, A. Jayaaraman, K.W. Wecht, D.L. Sivco, and A.Y. Cho, Appl. Phys. Lett. 52, 2124 (1988). [15] V.A. Wilkinson, A.D. Prins, J.D. Lambkin, E.P. OReilly, D.J. Dunstan, L.K. Howard, and M.T. Emeny, Phys. Rev. B 42, 3113 (1990).

DEFORMATION POTENTIALS

273

[16] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [17] Y. Zhang, A. Mascarenhas, H.P. Xin, and C.W. Tu, Phys. Rev. B 61, 4433 (2000). [18] M.H. Ya, Y.F. Chen, and Y.S. Huang, J. Appl. Phys. 92, 1446 (2002). [19] Y. Gonzalez, G. Armelles, and L. Gonzalez, J. Appl. Phys. 76, 1951 (1994). [20] K. Pelhos, S.A. Lee, Y. Rajakarunanayake, and J.L. Reno, Phys. Rev. B 51, 13256 (1995). [21] J.A. Sans and A. Segura, High Pressure Res. 24, 119 (2004). [22] A. Beliveau and C. Carlone, Phys. Rev. B 41, 9860 (1990). [23] W. Shan, W. Walukiewicz, J.W. Ager III, K.M. Yu, J. Wu, E.E. Haller, Y. Nabetani, T. Murakawa, Y. Ito, and T. Matsumoto, Appl. Phys. Lett. 83, 299 (2003). [24] E. Griebl, G.F. Sch€otz, C. Birzer, W. Kerner, T. Reisinger, B. Hahn, and W. Gebhardt, Acta Phys. Polon. A 88, 995 (1995). [25] W. Walukiewicz, W. Shan, K.M. Yu, J.W. Ager III, E.E. Haller, I. Miotkowski, M.J. Seong, H. Alawadhi, and A.K. Ramdas, Phys. Rev. Lett. 85, 1552 (2000). [26] J. Wu, W. Walukiewicz, K.M. Yu, W. Shan, J.W. Ager III, E.E. Haller, I. Miotkowski, A.K. Ramdas, and C.-H. Su, Phys. Rev. B 68, 033206 (2003). [27] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [28] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [29] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [30] T.R. Parker, C.C. Phillips, and P.C. May, Phys. Rev. B 51, 4264 (1995).

9 Heterojunction Band Offsets and Schottky Barrier Height 9.1 HETEROJUNCTION BAND OFFSETS 9.1.1 General Considerations One of the most important parameters for the design and analysis of heterojunction and QW electronic and optoelectronic devices is the heterojunction band offset. The band offset is a consequence of the difference between the band-gap energies of two semiconductors. As shown in Figure 9.1, the energy difference is distributed between a CB offset DEc and a VB offset DEv. In a type I (straddling lineup), we obtain DEg ¼ DEc þ DEv

ð9:1Þ

while for type II (broken-gap and staggered lineups) the relationship is given by DEg ¼ jDEc DEv j

ð9:2Þ

where DEg ¼ jEg1 Eg2j is the band-gap energy difference. Since the temperature variations of the band-gap energies are very similar among various semiconductors [1], the band offsets and offset ratio can usually be assumed to be independent of temperature.

9.1.2 Group-IV Semiconductor Heterostructure System (a) CSi/Si The CxSi1x/Si heterostructure shows a biaxial tensile strain in the alloy layer. The biaxial strain or stress in the coherently strained QW layers splits the LH and HH bands so that the LH band is highest in CxSi1x layer. Similarly, for CxSi1x layers with smaller x compositions, the lowest CB is at the X (D) band. Brunner et al. [2] measured near-band-edge emission from pseudomorphic CxSi1x/Si QW structures with x up to 2 at%. They found a linear decrease in the PL emission peak with increasing x, which is about 30% larger than the expected band-gap reduction induced by strain. This might indicate that incorporation of C reduces the intrinsic band-gap energy. The trend for decreasing CxSi1x band-gap energy was also proposed by detailed binding calculations [3]. The band-offset values for CxSi1x/Si heterostructure have been determined experimentally by several authors [4, 5]. Houghton et al. [4] confirmed a type-I alignment in CxSi1x/Si with x ¼ 0.5 1.7 at% and also observed an elastic-strain-induced transition from type I to type II in Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

276

PROPERTIES OF SEMICONDUCTOR ALLOYS (a)

(b)

(c)

ΔEc ΔEc

Eg1

ΔEv

Eg2 ΔEv

Figure 9.1 Schematic energy-band diagrams showing three representative types of heterostructure interfaces: (a) type I (straddling lineup), (b) type II-misaligned (broken-gap lineup) and (c) type IIstaggered (staggered lineup)

CxSi1x/Si QWs. The band-offset ratio obtained by these authors is DEc : DEv ¼ 65 : 35 with Eg(Si) Eg(CxSi1x). Williams et al. [5] also obtained a band-offset ratio of about 70 : 30 (a)

(b) ΔEc=0.3ΔEg ΔEc=0.7ΔEg

ΔEv=1.3ΔEg

ΔEv=0.3ΔEg Si

Cx Si1-x

Si

Six Ge1-x

Figure 9.2 Schematic energy-band alignments for (a) CxSi1x/Si and (b) SixGe1x/Si heterostructures obtained by Williams et al. [5] and Cheng et al. [12], respectively

for x ¼ 0.5 1.7 at%. The corresponding band lineup is shown schematically in Figure 9.2(a). An ab initio calculation confirms the offset ratio of 70 : 30 [6]. (b) SiGe/Si Previous studies on the band alignment of the SixGe1x/Si heterostructure suggest type-I [7, 8] or type-II behavior [9–12]. By employing a wafer bending technique, Thewalt et al. [11] observed both type-I and type-II behaviors respectively, in PL of an UHV-CVD-grown Si0.7Ge0.3/Si(100) QW at high and low laser powers. They concluded that a determination of type-I alignment [7, 8] is a result of the band-bending effects due to high excitation. More recently, Cheng et al. [12] made PL measurements on UHV-CVD-grown and MBE-grown SixGe1x/Si MQWs and concluded that the band alignment was type II with DEc ¼ 0.3DEg and DEv ¼ 1.3DEg, as shown in Figure 9.2(b). (c) CSiGe/Si The incorporation of C into SixGe1x can compensate for some of the biaxial compressive strain in the SixGe1x/Si heterostructure. The incorporation of C evidently lowers the CB and VB energies and decreases the intrinsic band gap in SixGe1x. The intrinsic band alignment of SixGe1x/Si is always type-II in character. Neglecting the effect of strain, therefore, we can

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

277

expect a transition from type II to type I by incorporating C into SixGe1x. In fact, Stein et al. [13, 14] and Hartmann et al. [15] concluded that the band alignment in the CxSiyGe1xy/Si heterostructure is type I, regardless of whether the strain is compensated or not. However, a staggered type-II alignment has been reported in strain-relaxed Ge-rich CxSiyGe1xy/Si heterostructures (x ¼ 0.01 0.02 and y ¼ 0.10 0.13), with electrons (holes) localized in the Si (CxSiyGe1xy) layer [16]. The band offsets DEc and DEv determined were typically 0.4 and 0.6 eV, respectively. (d) CSi/SiGe Using a wafer bonding technique, Houghton et al. [4] obtained a type-II transition in a C0.01Si0.99/Si0.84Ge0.16/Si heterostructure, with electrons (holes) localized in the C0.01Si0.99 (Si0.84Ge0.16) layer.

9.1.3 III–V Semiconductor Heterostructure System: Lattice-matched Ternary-alloy System (a) GaInP/GaAs The band-offset ratio DEc : DEv determined experimentally for the Ga0.52In0.48P/GaAs heterostructure ranges widely from 13 : 87 to 63 : 37 [17]. The mean offset ratio gives DEc : DEv ¼ 33 : 67. The corresponding band offsets are DEc 0.16 eV and DEv 0.33 eV. The existence of spontaneous ordering in the Ga0.52In0.48P layer could significantly alter the band offset [17]. Thus, it appears that the ordering effect itself might have contributed to the larger scatter in the reported values, at least to some extent. The ordering effect can also change the band alignment from type I to type II, as schematically shown in Figure 9.3. (a)

(b)

(c)

ΔEc =0.16 eV GaAs

1.43 eV

ΔEc =0.33 eV

Fully disordered Ga 0.52In 0.48P

Partly ordered Fully ordered Ga 0.52In 0.48P Ga 0.52In 0.48P

Figure 9.3 Schematic energy-band diagram showing the effect of spontaneous ordering for Ga0.52In0.48P/GaAs heterostructure

Zhang et al. [17] obtained theoretically a transition from type I to type II at h ¼ 0.46 (0.54) in the GaxIn1xP/GaAs heterostructure with x ¼ 0.50 (0.52), where h is the so-called order parameter. (b) GaInP/AlInP Patel et al. [18] obtained the band-offset ratio DEc : DEv ¼ 52 : 48 in the Ga0.52In0.48P/ Al0.5In0.5P heterostructure, where the CB minimum is in the X valley for Al0.5In0.5P and in

278

PROPERTIES OF SEMICONDUCTOR ALLOYS

the G valley for Ga0.52In0.48P (i.e. DEc ¼ EcX(Al0.5In0.5P) EcG(Ga0.52In0.48P)). More recently, Dawson et al. [19] revised the offset ratio to DEc : DEv ¼ 67 : 33 from low-temperature PL measurements. (c) GaInP/AlGaAs The band alignment in the Ga0.52In0.48P/AlxGa1xAs heterostructure is expected to change from a straddling to a staggered type as the Al content x increases from x ¼ 0 (GaAs), as shown in Figure 9.4. Kim et al. [20] reported a transition occurring at about x ¼ 0.12 (Figure 9.4(b)). (a)

(b)

(c)

ΔEc =0.16 eV

Ga 0.52In 0.48P GaAs (x=0)

x=0.12

x> 0.12

ΔEv =0.33 eV Ga 0.52In 0.48P/Al xGa 1-xAs

x

Figure 9.4 Schematic energy-band diagram for Ga0.52In0.48P/GaxAl1xAs heterostructure with (a) x ¼ 0, (b) x ¼ 0.12 and (c) x > 0.12

(d) AlGaAs/GaAs The pioneering work of Dingle et al. [21, 22] on the AlxGa1xAs/GaAs MQW structure gave the offset ratio of DEc : DEv ¼ 85 : 15. Although this ratio had long been accepted, some studies required different ratios in the range of (0.62 0.66) : (0.38 0.34) to explain electrical and photoelectric data. The discrepancy with Dingles result was attributed to compositional grading or any interface states at the AlxGa1xAs/GaAs heterojunction. However, in 1984 Miller et al. [23, 24] reported values of 51 : 49 and 57 : 43 using PL from parabolic and rectangular QWs. Subsequently, Dugan et al. [25] arrived at 65 : 35. By averaging the recently published data, we recommend an offset ratio of DEcG : DEv ¼ 63 : 37. Using this ratio and the E0 and EgX values shown in Table 6.11, we obtain the DEc and DEv versus x plots for the AlxGa1xAs/GaAs heterostructure. Figure 9.5 shows these results. We can see that the band lineup is type I over the whole composition range 0 x 1.0 [26]. Note, however, that the CB minimum changes from the G point ðDEcG Þ to the X point ðDEcX Þ at x 0.43. The band offsets can be finally approximated for x 0.8 as (in eV) DEcG ðxÞ ¼ 0:85x

ð9:3aÞ

DEcX ðxÞ ¼ 0:480:30x

ð9:3bÞ

DEv ðxÞ ¼ 0:50x

ð9:3cÞ

ΔEc (eV)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT 1.2 1.0 0.8 0.6 0.4 0.2 0

279

AlxGa1-xAs/GaAs

ΔEcX

ΔEcΓ

ΔEv (eV)

Eg(GaAs)=1.43 eV

0 -0.2 -0.4 -0.6 -0.8 0

ΔEv

0.2

0.4

x

0.6

0.8

1.0

Figure 9.5 A full AlxGa1xAs/GaAs heterostructure band diagram obtained by assuming a band-offset ratio of DEcG : DEv ¼ 63 : 37 and using E0 and EgX in Table 6.11 (solid lines). The dashed lines represent the linear variations of DEc and DEv given by Equation (9.3)

(e) AlInAs/InP The Al0.48In0.52As/InP interface is the least well characterized [27]. The staggered type-II alignment with holes localized in the Al0.48In0.52As layer is generally agreed upon. A CB offset of DEc ¼ 2.86DEg has been reported by B€ ohrer et al. [28]. The direct and inverse heterointerface properties have been studied for the Al0.48 In0.52As/InP heterostructure (Al0.48In0.52As layer grown on InP versus InP layer grown on Al0.48In0.52As) [29, 30]. The clear noncommutativity of 100 20 meV [29] and 53 10 meV [30] has been observed for DEc. (f) GaInAs/InP The band offsets in the Ga0.47In0.53As/InP heterostructure have been studied both theoretically and experimentally [27]. We obtain an averaged experimental offset ratio of DEc : DEv ¼ 38 : 62. The corresponding band alignment is shown in Figure 9.6(a). (b)

(a) ΔEc=0.27 eV

InP

Ga 0.47 In 0.53 As

ΔEv=0.45 eV

ΔEc=0.51 eV

Al 0.48 In 0.52 As

ΔEv=0.22 eV

Figure 9.6 Schematic energy-band alignments for (a) Ga0.47In0.53As/InP and (b) Ga0.47In0.53As/ Al0.48In0.52As heterostructures. The band offsets DEc and DEv are obtained by averaging the literature data

280

PROPERTIES OF SEMICONDUCTOR ALLOYS

The direct and inverse heterointerface properties have been studied on the Ga0.47In0.53As/ InP heterointerface [30, 31]. Substantially large noncommutativity has been reported. The cause of the noncomutativity is attributed to a difference in the chemical nature of the direct and inverse interfaces [31]. A significant nontransitivity for the average band offsets has also been found in the InPAlxIn1xAsGaxIn1xAs family [29, 30]. (g) GaInAs/AlInAs Like Ga0.47In0.53As, Al0.48In0.52As can be grown lattice-matched to InP. The band-gap difference DEg between these ternaries is about 0.73 eV. The band offsets in the Ga0.47 In0.53As/Al0.48In0.52As heterostructure have been determined by several authors [27, 32–34]. Averaging these results produces the offset ratio of DEc : DEv ¼ 70 : 30. The corresponding band lineup is shown in Figure 9.6(b). (h) InAsSb/GaSb InAs0.91Sb0.09 can be grown lattice-matched to GaSb. A broken type of band lineup is accepted for the InAs0.91Sb0.09/GaSb heterostructure [35–37]. Mebarki et al. [36] reported band offsets of DEc ¼ 0.82 eV and DEv ¼ 0.36 eV, respectively. The band lineup for this heterojunction system is illustrated in Figure 9.7.

GaSb

ΔEv =0.36 eV

ΔEc =0.82 eV

InAs0.91Sb0.09

Figure 9.7 Schematic energy-band diagram for InAs0.91Sb0.09/GaSb heterostructure obtained by Mebarki et al. [36]

9.1.4 III–V Semiconductor Heterostructure System: Lattice-matched Quaternary Alloy (a) GaInPAs/InP Although the straddling alignment is generally agreed upon, there is considerable disagreement regarding the band offsets of the GaxIn1xPyAs1y/InP heterostructure [27]. Let us assume a band-offset ratio of DEc : DEv ¼ 38 : 62, which is derived from the Ga0.47In0.53As/InP heterostructure. Using this ratio and E0 in Table 6.28, we obtain the y-dependent DEc and DEv values for the GaxIn1xPyAs1y/InP and GaxIn1xPyAs1y/Ga0.47In0.53As heterostructures. The results can be approximated as (in eV) DEc ðyÞ ¼ 0:230:23y

ð9:4aÞ

DEv ðyÞ ¼ 0:370:37y

ð9:4bÞ

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

281

for the GaxIn1xPyAs1y/InP heterostructure and DEc ðyÞ ¼ 0:23y

ð9:5aÞ

DEv ðyÞ ¼ 0:37y

ð9:5bÞ

for the GaxIn1xPyAs1y/Ga0.47In0.53As heterostructure. (b) AlGaAsSb/GaSb The band offsets in a perfectly lattice-matched Al0.47Ga0.53As0.04Sb0.96/GaSb heterostructure were determined to be DEc ¼ 0.35 eV and DEv ¼ 0.24 eV, respectively, furnishing a fractional ratio of DEc : DEv ¼ 59 : 41 [38]. (c) AlGaAsSb/InP Ostinelli et al. [39] carried out PL on an Al0.168Ga0.832AsSb/InP heterostructure and obtained staggered type-II offsets of DEc ¼ 0.32 eV and DEv ¼ 0.66 eV with electrons (holes) localized in the InP (Al0.168Ga0.832AsSb) layer. These results give DEc ¼ 0.94DEg and DEv ¼ 1.94DEg. (d) AlGaAsSb/InAs Nelson et al. [40] measured PL spectra of the Al0.8Ga0.2As0.14Sb0.86/InAs heterostructure and obtained a staggered lineup with DEc ¼ 1.60 eV and DEv ¼ 0.24 eV with electrons (holes) localized in the InAs (Al0.8Ga0.2As0.14Sb0.86) layer. These results predicted the relationship DEc ¼ 1.18DEg and DEv ¼ 0.18DEg. (e) GaInAsSb/GaSb The band lineup for GaxIn1xAsySb1y/GaSb heterostructure is believed to be type II in nature. Mikhailova and Titkov [41] reviewed the topic. Averaging the experimental data in this review gives DEc ¼ 1.62DEg and DEv ¼ 0.62DEg. These relationships indicate that the transition composition from broken-gap to staggered lineup will be at x 0.24. Afrailov et al. [42] observed a broken-gap character at x ¼ 0.11, whereas Mebarki et al. [43] found the staggered band offsets to be DEc ¼ 0.33 0.05 eV and DEv ¼ 0.12 0.05 eV (x ¼ 0.77) with electrons localized in the GaxIn1xAsySb1y layer. (f) GaInAsSb/InP The band-offset ratio of DEc : DEv ¼ 30 : 70 in the Ga0.64In0.36As0.84Sb0.16/InP heterostructure was obtained by Chang et al. [44] from optical absorption measurements. (g) GaInAsSb/InAs The band lineups in LPE-grown GaxIn1xAsySb1y/InAs heterostructure were investigated by Mikhailova et al. [45]. The broken-gap lineup was observed in the composition range 0.77 x 0.97 and the staggered lineup in the range 0 < x < 0.7.

282

PROPERTIES OF SEMICONDUCTOR ALLOYS

(h) AlGaAsSb/GaInAsSb The band offsets in the Al0.22Ga0.78As0.02Sb0.98/Ga0.75In0.25As0.04Sb0.96 MQW structure grown on GaSb(100) were determined from optical absorption and PL measurements [46]. The offset ratio was determined to be DEc : DEv ¼ 66 : 34. (i) AlInAsSb/GaInAsSb Chang et al. [47] grew Al0.66In0.34As0.85Sb0.15/Ga0.64In0.36As0.84Sb0.16 MQW structures on InP (100) by MOCVD and carried out low-temperature PL measurements. The band-offset ratio estimated from this study was DEc : DEv ¼ 75 : 25. (j) AlGaInP/AlInP The band alignment in (Al0.7Ga0.3)0.53In0.47P/AlxIn1xP heterostructures was investigated by Ishitani et al. [48] using PL spectroscopy. They found that the X-valley discontinuity DEcX decreases with increasing x (0.47 x 0.61). The band-offset ratio obtained was DEc : DEv ¼ 75 : 25 for x ¼ 0.53. (k) AlGaInP/GaInP

ΔEv (eV)

ΔEc (eV)

The band-offset ratios in (AlxGa1x)0.53In0.47P/Ga0.52In0.48P with x in the direct band-gap region (x < 0.65, see Figure 6.49) varied from DEcG : DEv ¼ 49 : 41 to 70 : 30 [49–53]. Averaging these data gives DEcG : DEv ¼ 65 : 35. The corresponding band offsets DEcG , DEcX and DEv are plotted against x in Figure 9.8. The band offsets can now be written as (in eV)

0.6 0.5 0.4 0.3 0.2 0.1 0 0 -0.1 -0.2 -0.3 0

DEcG ¼ 0:43x

ð9:6aÞ

DEcX ¼ 0:360:16x

ð9:6bÞ

DEv ¼ 0:24x

ð9:6cÞ

(AlxGa1-x)0.53In0.47P/Ga0.52In0.48P

ΔEcX

ΔEcΓ Eg~1.9 eV (Ga0.52In0.48P)

ΔE v

0.2

0.4

x

0.6

0.8

1.0

Figure 9.8 A full (AlxGa1x)0.53In0.47P/Ga0.52In0.48P heterostructure band diagram obtained by assuming a band-offset ratio of DEcG : DEv ¼ 65 : 35 and using E0 and EgX in Table 6.28 (solid lines). The dashed lines represent the linear variations of DEc and DEv given by Equation (9.6)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

283

The band offsets in (AlxGa1x)0.53In0.47P/Ga0.52In0.48P with x in the indirect band-gap region were studied by several authors [54, 55]. The effects of long-range ordering on the band alignment are discussed by Shao et al. [56]. (l) AlGaInAs/GaInAs

ΔEv (eV)

ΔEc (eV)

The band offsets in (AlxGa1x)0.48In0.52As/Ga0.47In0.53As were determined from I V [57] and PL and PLE measurements [58]. The offset ratios determined from these studies were DEc : DEv ¼ 72 : 28 and 73 : 27, respectively. Assuming DEc : DEv ¼ 73 : 27 and using E0 in Table 6.28, we can obtain the x-dependent DEc and DEv. The results are shown in Figure 9.9, and can be given by (in eV)

0.6 0.5 0.4 0.3 0.2 0.1 0 0 -0.1 -0.2 -0.3 0

DEc ðxÞ ¼ 0:54x

ð9:7aÞ

DEv ðxÞ ¼ 0:20x

ð9:7bÞ

(AlxGa1-x)0.48In0.52As/Ga0.47In0.53As ΔEc

Eg~0.75 eV (Ga0.47In0.53As) ΔEv

0.2

0.4

x

0.6

0.8

1.0

Figure 9.9 A full (AlxGa1x)0.48In0.52As/Ga0.47In0.53As heterostructure band diagram obtained by assuming a band-offset ratio of DEc : DEv¼73 : 27 and using E0 in Table 6.28

9.1.5 III–V Semiconductor Heterostructure System: Lattice-mismatched Alloy System (a) w-AlGaN/w-GaN The straddling lineup is generally agreed upon, but there is considerable disagreement regarding the band offsets between AlxGa1xN (AlN) and GaN reported by different authors [59–65]. Using the mean value of these data, we obtain DEc : DEv ¼ 65 : 35. Using E0 ¼ 6.2 eV (AlN) and 3.420 eV (GaN) in Table 6.2, we obtain the band offsets for the AlxGa1xN/GaN heterostructure as follows (in eV) DEc ðxÞ ¼ 1:81x

ð9:8aÞ

DEv ðxÞ ¼ 0:97x

ð9:8bÞ

284

PROPERTIES OF SEMICONDUCTOR ALLOYS

Dependence of the AlN/GaN band discontinuity on growth temperature was determined using XPS [66]. A large strain-induced asymmetry of the band offset was suggested from an ab initio electronic structure study [67]. (b) w-AlInN/w-InN The VB offsets DEv ¼ 3.10 0.04 eV [68] and 4.0 0.2 eV [69] were determined in an AlN/ InN heterointerface using photoelectron spectroscopy. These DEv values and values of E0 ¼ 6.2 eV (AlN) and 0.70 eV (InN) in Table 6.2 provide the band-offset ratios DEc : DEv 44 : 56 and 27 : 73, respectively. (c) w-GaInN/w-GaN The band offsets in the GaxIn1xN(InN)/GaN heterostructure were determined using various techniques [70–74]. The mean offset ratio obtained from these studies was DEc : DEv ¼ 67 : 33. (d) GaInAs/GaAs The band discontinuity in a strained-layer system depends not only on the heterostructure system involved but also on the amount of mismatch strain at the interface. The strain field can produce marked effects on the electronic properties through the DP interactions. The hydrostatic component of the strain causes a shift in the bulk energy levels of the strained layer, while the shear component causes splitting of certain degenerate VB levels, namely, the HH and LH levels. The exact energy levels of the heterostructure layer should, therefore, be determined including the strain modification of the layer. In the case of biaxial strain parallel to [010] and [001], the strain components in GaxIn1xAs/ GaAs(100) heterojunctions are exx ¼ eyy ¼ d; ezz ¼

2C12 d; exy ¼ eyz ¼ ezx C11

with d¼

Da a

ð9:9Þ

ð9:10Þ

where d is defined to be positive for compressive strain, Cij is the elastic stiffness constant of GaxIn1xAs and Da is the lattice-constant difference between GaxIn1xAs and GaAs. The corresponding change in the band-gap energy for GaxIn1xAs layer can be written as DEc;v1 ¼ DEc;v2 ¼

2aG0

C11 C12 C11 þ 2C12 1 þb d ¼ dh þ dEs 2 C11 C11

C11 C12 C11 þ 2C12 1 2aG0 b d ¼ dh dEs 2 C11 C11

ð9:11aÞ ð9:11bÞ

where v1 and v2 represent the j3/2, 3/2> (HH-like) and j3/2, 1/2> (LH-like) bands, respectively, aG0 and b are the hydrostatic-pressure and shear DPs, respectively. In obtaining Equation (9.11), the SO split-off energy D0 is assumed to be D0 dEs. Introducing the InAs (x ¼ 0)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

285

values for aG0 , b and Cij (d ¼ 0.07) into Equation (9.11), we obtain the hydrostatic-pressure and shear-strain shifts dh and dEs in the strained InAs layer to be about 0.40 and 0.26 eV, respectively. Thus, the band-gap discontinuity between GaAs and fully strained InAs is DE0 ¼ E0 ðGaAsÞ½E0 ðInAsÞ þ dh 1:43ð0:36 þ 0:40Þ ¼ 0:67 eV

ð9:12Þ

Similarly, the discontinuity between GaAs and fully relaxed InAs is given by DE0 ¼ E0 ðGaAsÞE0 ðInAsÞ 1:430:36 ¼ 1:07 eV

ð9:13Þ

The InAs/GaAs heterostructure has about 7% lattice mismatch and the corresponding critical thickness is as low as two monolayers. Using XPS, Kowalczyk et al. [75] determined the band offsets in the InAs/GaAs(100) heterostructure to be DEc ¼ 0.90 0.07 eVand DEv ¼ 0.17 0.07 eV, respectively. The resulting offset ratio is DEc : DEv ¼ 16 : 84. The sample used by Kowalczyk et al. [75] was an InAs/GaAs(100) single heterojunction with a 20 A thick InAs layer, which is much thicker than the critical thickness for the generation of dislocation. Hence, the lattice strain is relaxed in their sample. In fact, the obtained band-gap discontinuity DE0 ¼ DEc þ DEv ¼ 1.07 eV exactly agrees with that predicted from Equation (9.13). If we assume an offset ratio of DEc : DEv ¼ 16 : 84 for the fully relaxed GaxIn1xAs/GaAs heterostructure, we can obtain the x-dependent offsets DEc and DEv (in eV) DEc ðxÞ ¼ 0:17x

ð9:14aÞ

DEv ðxÞ ¼ 0:90x

ð9:14bÞ

The largest d and DE0 values can be expected at x ¼ 0 for the strained GaxIn1xAs/GaAs heterostructure. Since both d and DE0 E0(GaAs) E0(GaxIn1xAs) for the strained GaxIn1xAs/GaAs heterostructure decrease almost linearly with increasing x, the hydrostatic component (dh) to DE0 ratio may be roughly independent of x and is given by dh/DE0 0.4 (0.40/1.07 at x ¼ 0). There are no experimental data on the band offsets in strained GaxIn1xAs/GaAs heterostructures for lower x values, except for x ¼ 0. Samples of larger x reported recently [27, 76–78] give a mean band-offset ratio of DEc : DEv ¼ 60 : 40 (0.6 < x 0.98). Using this ratio and the strained-InAs (x ¼ 0) E0 value, we can obtain an energy-band diagram for the strained GaxIn1xAs/GaAs heterostructure. This result is shown in Figure 9.10. The band offsets DEc,

ΔEc=0.48 eV GaAs GaAs (x=1.0) 0.63 eV

InAs (x=0) 0.76 eV 0.13 eV (HH-like) 0.13 eV (LH-like)

Ga In x

x 1-x

As/GaAs

ΔEv1=0.32 eV ΔEv2=0.06 eV

Figure 9.10 Schematic energy-band diagram for strained GaxIn1xAs/GaAs heterostructure obtained by using a band-offset ratio of DEc : DEv ¼ 60 : 40 and strained-InAs E0 value of 0.76 eV

286

PROPERTIES OF SEMICONDUCTOR ALLOYS

DEv1 (CB HH) and DEv2 (CB LH) versus x can be written as (in eV) DEc ðxÞ ¼ 0:48x

ð9:15aÞ

DEv1 ðxÞ ¼ 0:32x

ð9:15bÞ

DEv2 ðxÞ ¼ 0:06x

ð9:15cÞ

(e) Dilute-nitride-based heterostructure system 1. GaNAs/GaAs—Recent experimental studies suggest that the band lineup in the dilutenitride GaNxAs1x/GaAs heterostructure for N 4.5 at% is type I [79–83], although an earlier XPS study suggested a type-II lineup [84]. The schematic band diagram for this heterostructure system is shown in Figure 9.11. It is commonly accepted that N incorporation mainly affects the CB states and causes band-gap reduction (Section 6.3.5). Based on the BAC model, the N states produced in GaAs lead to a characteristic splitting of the G6-CB state into two non-parabolic subbands E and E þ (Figure 9.11(b), see also Figure 6.29(b)). The different lattice constants between c-GaN and GaAs can induce tensile strain parallel to [010] and [001] in pseudomorphic GaNxAs1x layers on GaAs(100) (Figure 1.27). This strain argument predicts that the LH band should be type I, while the HH band is type II, as illustrated in Figure 9.11(c). The CB offsets DEc ¼ (0.7 0.95)DEg were reported [79–83]. (a)

(b)

(c) E+

CB ΔE c

E-

ΔE v2(LH-like) VB GaAs

Ga N As x

1-x

ΔE v1 (HH-like) Ga N As x

1-x

GaAs

Figure 9.11 Schematic energy-band diagram for GaNxAs1x/GaAs heterostructure. Strain argument depicted in (c) predicts the LH and HH bands to be type I and type II, respectively

2. GaInNAs/GaAs—The schematic energy-band diagram for the dilute-nitride GaxIn1xNyAs1y/ GaAs heterostructure is shown in Figure 9.12. As mentioned in Section 9.1.4, the band-offset ratios in fully relaxed and strained GaxIn1xAs/GaAs heterostructures are assumed to be given by DEc : DEv ¼ 16 : 84 and 60 : 40, respectively. The band lineup in Figure 9.12(a) corresponds to the strained heterostructure. Strain-induced splitting of the HH and LH bands cannot be expected in the fully relaxed heterostructure system. Adding N to GaxIn1xAs splits the CB minimum into E and E þ and lowers the band-gap energy, with negligible interaction with the

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT (a)

287

(b) ΔE c

CB

E+ EΔEv1 (HH-like)

VB ΔEv2 (LH-like) GaAs

GalnAs

GalnNAs

Figure 9.12 Schematic energy-band diagrams for strained heterostructure systems: (a) GaxIn1xAs/ GaAs and (b) dilute-nitride GaxIn1xNyAs1y/GaAs

VB states (Figure 9.12(b)). We can, thus, expect an increase (decrease) in the DEc (DEv) portion. Indeed, the band discontinuities have been found to be 80% in the CB and 20% in the VB for GaxIn1xNyAs1y/GaAs heterostructures [85, 86]. 3. GaNAsSb/GaAs—As seen in Figure 9.11(b), incorporating N into GaAs essentially lowers the CB minimum. This is complementary to the Sb effect, which mainly increases the VB maximum. In this respect, the GaNxAsySb1xy/GaAs heterostructure is an interesting system where DEc and DEv can be independently tuned by adjusting N and Sb concentrations, respectively. The band discontinuities in this heterostructure system have been studied by several authors [87–90] and are found to change from type II to type I by incorporating N into GaAsxSb1x.

9.1.6 II–VI Semiconductor Heterostructure System (a) (II, II)–O-based heterostructure system The band alignment in the Mg0.15Zn0.85O/CdS heterostructure was studied using X-ray and UV photoelectron spectroscopy and found to be a staggered type-II alignment with electrons localized in the Mg0.15Zn0.85O layer (DEc ¼ 1.1 eV and DEv ¼ 1.2 eV) [91]. The XPS technique was used to obtain the band offsets in the Zn0.95Cd0.05O/ZnO(0001) heterostructure [92]. The band offsets obtained were DEc ¼ 0.30 eV and DEv ¼ 0.17 eV, with electrons and holes localized in the Zn0.95Cd0.05O layer (type I). (b) (II, II)S-based heterostructure system The band offsets in free-standing c-Zn0.7Cd0.3S/c-ZnS SL were determined from lowtemperature PL to be DEc ¼ 0.461 eV and DEv ¼ 0.088 eV (DEc : DEv ¼ 84 : 16) [93]. (c) (II, II)Se-based heterostructure system The band alignments in ZnSe-based heterostructures, such as BexZn1xSe/ZnSe, MgxZn1xSe/ ZnSe and ZnxCd1xSe/ZnSe, are type I. From magneto-transmission measurements on a series

288

PROPERTIES OF SEMICONDUCTOR ALLOYS

of BeZnSe/ZnMnSe QWs, Kim et al. [94] estimated the VB offset in BexZn1xSe/ZnSe to be approximately 40% of the band-gap difference. The VB offset in the MgxZn1xSe/ZnSe heterostructure was determined from optical and photoelectron spectra to be as much as 87% of the band-gap difference [95]. The band offsets in the ZnxCd1xSe/ZnSe heterostructure were determined using various techniques, such as optical absorption [96], reflectance [97], electrical conductivity and intersubband absorption [98], PLE [99] and CL and DLTS [100]. These data gave a band-offset ratio which varied from DEc : DEv ¼ 67 : 33 to 87 : 13. We obtained DEc : DEv ¼ 72 : 28 as the average band-offset ratio. Guenaud et al. [99] reported that the HH excitons are type I, whereas the LH excitons are type II. The type-II excitons were considered to occur as a result of the compressive strain state and to have small VB offset (DEc : DEv ¼ 87 : 13) in the ZnxCd1xSe/ZnSe (x ¼ 0.82 0.88) heterostructure. The band offsets in the ZnxCd1xSe/MgSe heterostructure have also been studied [101]. (d) (II, II)Te-based heterostructure system It is generally accepted that the strained ZnxCd1xTe/CdTe heterostructure is of mixed type, i.e. the electrons and heavy holes are confined in a CdTe layer, while the light holes are confined in a ZnxCd1xTe layer [102–105]. This is the result of sufficient residual tensile strain existing in the ZnxCd1xTe layer grown on ZnyCd1yTe (x > y). Similarly, band alignments of type I and type II have been observed in ZnxCd1xTe/ZnTe heterostructures below and above x 0.1 respectively, grown on GaAs(100) [106]. The electrons and holes in type II can be confined in the ZnxCd1xTe and ZnTe layers, respectively. The VB offset between CdTe and HgTe has been the subject of a number of investigations. In early experiments, both a small offset of 40 meV and a roughly 10 times larger value were deduced (see von Truchseb et al. [107]). However, more recent experiments using various techniques provide consistent VB offsets somewhere around 0.4 eV [108–113]. The most recent study gives temperature-dependent offset data of DEv ¼ 0.57 0.06 eV at 5 K and its temperature coefficient dDEv/dT 0.4 meV/K [114]. Strong evidence has also been provided to suggest that the temperature dependence of the band offsets can be essentially neglected [112]. Figure 9.13 shows the schematic band diagram for the CdxHg1xTe/CdTe heterostructure. The HgTe/CdTe lineup corresponds to that reported by Becker et al. [114]. The results

CdTe/CdTe

CdTe/CdxHg1-xTe

CdTe/HgTe

Γ6 Electron

Γ8

E0=1.51 eV

Hole

Γ8 x

ΔEc =1.21 eV

Γ6

E0 =-0.15 eV

ΔE v = 0.45 eV

Figure 9.13 Schematic energy-band diagram for CdxHg1xTe/CdTe heterostructure. The HgTe/CdTe lineup corresponds to that reported by Becker et al. [114] at 300 K. The band offsets can be written as Equation (9.16)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

289

suggest that the band offsets can be expressed as (in eV) DEc ðxÞ ¼ 1:211:21x

ð9:16aÞ

DEv ðxÞ ¼ 0:450:45x

ð9:16bÞ

Thus, the CdxHg1xTe/CdTe heterostructure is type II (x ¼ 0) and becomes type I for x > 0.09. (e) Zn(VI, VI)-based heterostructure system Shahzad et al. [115] carried out PL and PLE measurements on ZnSxSe1x/ZnSe SLs (x 0.26) and obtained a very small CB offset (10 meV) between ZnSe wells and ZnSxSe1x barriers with a type-I lineup. Subsequently, Lomascolo et al. [116] undertook PL measurements on a ZnS0.18Se0.82/ZnSe SL at hydrostatic pressures up to 8 GPa and confirmed a transition from type I to type II near 4.5 GPa. The CB offset estimated in this study was DEc 6 meV at zero pressure. We can thus conclude that the band-offset ratio for ZnSxSe1x/ZnSe heterostructure is roughly given by DEc : DEv ¼ 0 : 100. ZnSe/ZnTe is known to comprise a staggered type-II heterostructure. The same band alignment can be expected and has been confirmed in ZnSexTe1x/ZnSe and ZnSexTe1x/ZnTe heterostructures [117, 118]. (f) (II, II)VI-based and II(VI, VI)-based heterostructure systems The band offsets in MgZnSe/ZnCdSe and ZnCdSe/ZnSSe heterostructures were determined experimentally by Pelucchi et al. [119] and Wu et al. [120], respectively. (g) (II, II)(VI, VI)-based heterostructure system The band lineup for MgxZn1xSySe1y/ZnSe heterostructure is believed to be type I. The bandoffset ratio was studied experimentally by several authors [121–126]. These studies provided offset ratios which varied largely from DEc : DEv ¼ 10 : 90 [124] to 60 : 40 [122]. We obtained DEc : DEv ¼ 36 : 64 as the mean value. The band offsets in Zn0.7Cd0.3S0.06Se0.94/ZnS0.06Se0.94 lattice-matched to GaAs have been characterized by DLTS [127] and the band-offset ratio obtained was DEc : DEv ¼ 75 : 25. (h) (II, II, II)VI-based heterostructure system The band alignment in BexMgyZn1xySe/ZnSe grown on GaAs(100) was investigated using PL and PLE [128] and the band-offset ratio was found to be DEc : DEv ¼ 60 : 40. The band offsets in Mg0.50Zn0.27Cd0.23Se/Zn0.53Cd0.47Se lattice-matched to InP were investigated using contactless ER [129]; the offset ratio was determined to be DEc : DEv ¼ 82 : 18 (DEc ¼ 0.59 eV).

9.2 SCHOTTKY BARRIER HEIGHT 9.2.1 General Considerations A Schottky barrier is a metal/semiconductor junction which has rectifying characteristics. Rectifying properties depend both on the metal work function and type of conductivty of

290

PROPERTIES OF SEMICONDUCTOR ALLOYS

the semiconductor. The choice of a metal for fabricating the Schottky barrier with a particular semiconductor is, thus, determined by its electronic work function fM. For an n-type semiconductor, fM should be large, while for a p-type semiconductor, it should be less than the electron affinity xe of the semiconductor. The barrier heights can then be written, respectively, as n-type : fn ¼ fM xe

ð9:17aÞ

p-type : fp ¼ Eg fM þ x e

ð9:17bÞ

where Eg is the band-gap energy of the semiconductor. The maximum value of the barrier height for an ideal SchottkyMott contact is about equal to the band-gap energy of the semiconductor: fn þ fp ¼ Eg. The work functions fM of some important metals used as the Schottky contacts are summarized in Table 9.2 of Adachi [1].

9.2.2 Group-IV Semiconductor Alloy (a) SiGe binary alloy

0.9 0.8 0.7 0.6 0.5 0.4 0.7

1.2 Metal/SixGe1-x

(a)

(c) 1.1

φn+φp , EgX (eV)

φp (eV)

φn (eV)

Extended studies on metal/SixGe1x have shown the complexity of the mechanism of Schottky barrier formation [130]. The results are still puzzling. However, a common trend has been observed: the Schottky barrier height fp increases with increasing x. The experimental data for fn and fp obtained by Aubry-Fortuna et al. [130] is shown in Figure 9.14. These authors observed that for lower-fM metals (Zr and Ti), fn decreases with x, while fp increases. For a higher fM metal (Pt), fn greatly increased. In the intermediate-fM metal (W), fn exactly follows the increase of Eg in SixGe1x with x, while fp remains constant. Nevertheless, whatever the metal, the sum fn þ fp gives the Eg variation as a function of x (Equation (9.17)), and the Fermi level is located at the same position for both n- and p-type layers. Figure 9.14(c)

Lower-φM Intermediate-φM Higher-φM

0.6 0.5 0.4 0.3 0.4

1.0 0.9 0.8

EgX

(b) 0.5

φn+φp (lower-φM)

0.6

0.7 x

0.8

0.9

1.0

0.7 0.4 0.5 0.6 0.7 0.8 0.9 1.0 x

Figure 9.14 Schottky barrier heights (a) fn and (b) fp for metal/SixGe1x contacts. The experimental data are taken from Aubry-Fortuna et al. [130]. The sum fn þ fp for the lower-fM metals, together with the band-gap energy EgX (Figure 6.8), are plotted against x in (c)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

291

shows a comparison of the sum fn þ fp for the lower-fM metals plotted in Figures 9.14(a) and 9.14(b) with the variation in EgX with x in SixGe1x (Figure 6.8). As for metal/Si and metal/Ge contacts [1], the results in Figure 9.14(c) suggest that the Schottky barrier height for metal/ SixGe1x contact exhibits the SchottkyMott contact nature very well. (b) CSiGe ternary alloy The Schottky barrier height on CxSiyGe1xy has been studied by several authors [130]. Adding C to SiGe leads to an increase in the W or Ti/p-type Schottky barrier height which is larger than that of the band-gap energy Eg, showing a change in the Fermi level position. Nevertheless, as in the case of SixGe1x, a weaker dependence on fM compared to that of Si is observed. High values of the ideality factor with increasing C content have also been observed.

9.2.3 III–V Semiconductor Ternary Alloy (a) (III, III) N alloy The Schottky rectifier properties of n-AlxGa1xN have been studied using various metal contacts. The Schottky barrier height fn versus x obtained by depositing Au, Ni and Pd metals on n-AlxGa1xN is shown in Figure 9.15. The experimental data are taken from various sources [131–135]. These plots suggest that it is difficult to establish an ideal Schottky contact and, thus, to obtain simple relationships such as that shown in Equation (9.17). This may be due to interface states caused by surface reactions of metal and semiconductor atoms and/or to any effects of crystalline imperfection. The n-AlxGa1xN samples plotted in Figure 9.15 were epitaxially grown on sapphire [131, 132, 134, 135] or on 6H-SiC substrate [133]. 1.8

1.8 (a) I-V

(b) C-V Au Ni Pd

1.4

1.6

φn (eV)

φn (eV)

1.6

1.2

1.4 1.2

1.0

1.0

0.8

0.8

0.6

0

0.1

0.2 x

0.3

0.6

Metal/AlxGa1-xN

0

0.1

0.2

0.3

x

Figure 9.15 Schottky barrier height fn versus x for samples with Au, Ni and Pd metals deposited on nAlxGa1xN: (a) I Vand (b) C V measurements. The experimental data are taken from various sources (see text)

Zhang et al. [136] reported the x-dependent breakdown voltage in an n-AlxGa1xN Schottky rectifier. The breakdown voltage increased from 2.3 kV for x ¼ 0 (GaN) to 4.3 kV for x ¼ 0.25. They also demonstrated that the use of p þ guard rings is effective in preventing premature edge breakdown.

292

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b) (III, III)P alloy

1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

3.0 (a)

2.7

(c)

2.4

φn+φp , Eg (eV)

φp (eV)

φn (eV)

Figure 9.16 shows the experimental fn and fp values for Au/GaxIn1xP Schottky barriers obtained by several authors [137–139]. The GaP and InP values are taken from Adachi [1]. The barrier height fn in Figure 9.16(a) increases almost linearly with increasing x, while fp in Figure 9.16(b) shows no strong dependence on x. The sum of fn and fp, together with E0 and EgX , are plotted against x in Figure 9.16(c). The Au/GaxIn1xP rectifiers show Schottky– Mott-like characteristics.

Au/GaxIn1-xP

E Xg

2.1 1.8 1.5

E0

1.2

0

φn+φp

0.9

(b) 0.2

0.4

x

0.6

0.8

1.0

0.6 0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.16 Schottky barrier heights (a) fn and (b) fp for Au/GaxIn1xP contacts. The experimental data are taken from various sources (see text). The open squares in (a) and (b) represent the endpoint binary data in Adachi [1]. The sum fn þ fp, together with E0 and EgX (Table 6.10), are plotted against x in (c)

The Schottky barrier heights for the common III–V and II–VI semiconductors allow a pattern in which the barrier height of p-type semiconductors (fp) can be determined solely by the anion of the semiconductor [140]. The corresponding barrier height of n-type semiconductors (fn) may be determined from the relationship of fn þ fp ¼ Eg. Hence, the difference in the barrier heights of the two n-type semiconductors with the same anion is equal to the difference in the band-gap energies between them. In Figure 9.16(b), we can see that the Au/ GaxIn1xP system obeys this rule, namely, the ‘common anion’ rule. The dependence of x on the Schottky barrier height fn for Ti/Pt/Au metals on AlxIn1xP (0 < x < 0.5) has been studied using IV and CV measurements [141]. The results obtained suggest that fn increases almost linearly with x at a rate of 14 meV/at%[Al]. This value is slightly smaller than that of E0, 22 meV/at%[Al] (Table 6.9). Thus, the metal/AlxIn1xP system may not obey the common anion rule (i.e. fp is dependent of x). (c) (III, III)As alloy 1. AlGaAs—The fn and fp values as a function of x for Al/AlxGa1xAs Schottky system have been plotted in Figure 9.17. The experimental data are taken from Adachi [26]. The solid lines in Figures 9.17(a) and 9.17(b) show the linear fits of these data (in eV) fn ðxÞ ¼ 0:77 þ 0:84x ð0 x 0:425Þ

ð9:18aÞ

fn ðxÞ ¼ 1:220:22x ð0:45 < x 1:0Þ

ð9:18bÞ

1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

293

3.0 φn+φp

2.7

E0, EgX

φn+φp , Eg (eV)

φp (eV)

φn (eV)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

Al/AlxGa1-xAs

(a)

(b)

2.4 2.1

X

Eg

1.8 E0

1.5

I-V C-V

0

0.2

0.4

0.6

0.8

1.2 0

1.0

x

(c) 0.2 0.4 0.6 0.8 1.0 x

Figure 9.17 Schottky barrier heights (a) fn and (b) fp for Al/AlxGa1xAs contacts. The experimental data are taken from Adachi [26]. The solid lines in (a) and (b) show the linear least-squares fits of Equation (9.18). The sum fn þ fp, together with E0 and EgX (Table 6.11), are plotted against x in (c)

fp ðxÞ ¼ 0:64 þ 0:52x

ð9:18cÞ

It can be easily seen from Equation 9.18(c) that the Al/AlxGa1xAs system does not obey the common anion rule. However, the sum of fn and fp plotted in Figure 9.17(c) is almost equal to the fundamental absorption edge E0 (or EgX ). The x-dependent Schottky barrier heights fn and fp in Figure 9.17 resemble those of the CB and VB offsets (DEc, DEv) shown in Figure 9.5. Tersoff [142] pointed out that the band lineups at semiconductor heterojunctions are simply correlated with the difference in the Schottky barrier heights formed by using the same metal on the semiconductors of the heterojunction pair. In essence, this means that the physical mechanism responsible for determining the Fermi level in Schottky barrier formation also determines the band lineups in heterostructures. 2. AlInAs—Figure 9.18 shows the fn and fp values plotted as a function of x for Al/AlxIn1xAs Schottky system. The experimental data are taken from various sources [143–145]. 3.0 φn+φp

(a)

φn (eV)

2.4

φn+φp , Eg (eV)

1.8 1.5 1.2 0.9 0.6 0.3 0 -0.3 1.8 1.5 1.2 0.9 0.6 0.3 0

φp (eV)

(b)

1.2

0.4

0.6 x

0.8

E0

(c)

Al/AlxIn1-xAs 0.2

EgX

1.8

0.6

0

X

E0, Eg

1.0

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.18 Schottky barrier heights (a) fn and (b) fp for Al/AlxIn1xAs contacts. The sum fn þ fp, together with E0 and EgX (see Table 6.13), are plotted against x in (c)

294

PROPERTIES OF SEMICONDUCTOR ALLOYS

The AlAs and InAs data are obtained from Adachi [146]. No experimental data has been reported for the Al/p-InAs Schottky barrier height (fp). In Figure 9.18(b), therefore, we plot the experimental fp for Au/p-InAs contact [146]. It should be noted that any metal/n-InAs (x ¼ 1.0) contact usually shows Ohmic behavior (i.e. fn 0 eV) [146]. The fp versus x plots in Figure 9.18(b) suggest that the Al/AlxIn1xAs system does not obey the common anion rule. However, the simple relationship fn þ fp E0ðEgX Þ holds in Figure 9.18(c). 3. GaInAs—The Schottky barrier height fn for Au/GaxIn1xAs contact has been determined using IV and CV measurements [147]. Figure 9.19 shows the results of these 1.2

φn (eV)

0.9

Au/GaxIn1-xAs

0.6 0.3 0 Ohmic

-0.3 0

0.2

0.4

0.6

0.8

1.0

x

Figure 9.19 Schottky barrier height fn for Au/GaxIn1xAs contact. The experimental data are taken from Adachi [1] (open squares) and Kajiyama et al. [147] (solid circles). The solid line shows the quadratic least-squares fit of Equation (9.19). The negative fn sign for x 0.15 indicates the downward bending of the CB at the interface (Ohmic contact)

measurements. The solid line represents the quadratic least-squares fit of the experimental data (in eV) fn ¼ 0:03 þ 0:05x þ 0:95x2 ð9:19Þ The Au/GaxIn1xAs contact is predicted to be Ohmic for x 0.15 (fn 0 eV). The negative fn sign stands for the downward bending of the CB at the interface. A Schottky barrier height of fn 0.2 eV is predicted for metal/n-Ga0.47In0.53As latticematched to InP. The barrier height control is an important tool in fabricating various devices. Diode engineered for high barrier height systematically showed a higher thermal stability than low-barrier diodes. Many attempts have therefore been made to enhance the barrier height of n-GaxIn1xAs by inserting various thin interlayers between the metal and n-GaxIn1xAs layer. Such interlayers were counter-doped p þ -GaxIn1xAs, n-InP, p-InP, n-GaAs, n-GaxIn1xP at different thickness and dopant densities, etc. [148, 149]. An effective barrier height up to fn 0.7 eV has been achieved. (d) (III, III)Sb alloy Figures 9.20(a) and 9.20(b) show the Shottky barrier height fn for Au/AlxGa1xSb and Au/ GaxIn1xSb contacts, respectively. The experimental data are taken from Chin et al. [150] and Keeler et al. [151], respectively. The solid line in Figure 9.20(a) shows the linear least-squares fit of the experimental data and provides fn 1.02 eV for Au/AlSb (x ¼ 1.0) contact. The

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT 1.2

1.2 (a) Au/AlxGa1-xSb

(b) Au/GaxIn1-xSb 0.9

φn (eV)

φn (eV)

0.9

0.6

0.3

0

295

0.6

0.3

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.20 Schottky barrier height fn for (a) Au/AlxGa1xSb and (b) Au/GaxIn1xSb contacts. The experimental data in (a) are taken from Chin et al. [150] and in (b) from Keeler et al. [151]. The open squares in (a) and (b) represent the endpoint binary data taken from Adachi [1]. The solid line in (a) shows the linear least-squares fit and estimates fn 1.02 eV for Au/AlSb contact

barrier height fp for Au/AlSb is 0.56 eV [1]. The sum fn þ fp 1.58 eV for Au/AlSb contact is, thus, slightly smaller than the AlSb band-gap energy EgX ¼ 1:615 eV (Table 6.1). The Schottky barrier height for Au/GaxIn1xSb can be expected to be fp 0 eV (i.e. Ohmic) [1]. Note, however, that Keeler et al. [151] obtained 0.017 fp 0.022 eV for Au contacts on p-GaxIn1xSb (0.62 x 0.905) layers. (e) Ga(V, V) alloy GaP0.35Sb0.65 is an InP lattice-matched material. In order to overcome the low value of the Schottky barrier height on n-InP (fn 0.4 eV [1, 146]), Loualiche et al. [152] fabricated a Au/ GaP0.35Sb0.65 Schottky barrier on InP and obtained a value of fn 0.6 eV. This value is the highest ever reported on InP lattice-matched materials that do not contain aluminum. The Schottky barrier height fn for Au/GaAsxSb1x contact has been determined using I–V and C–V measurements [153]. Figure 9.21 shows these results, together with the x dependence

1.8

1.8 1.5

Au/GaAsxSb1-x

1.2

1.2 E0

0.9 0.6

0.6

φn

0.3 0

0.9

0

0.2

0.4

x

0.6

E0 (eV)

φn (eV)

1.5

0.3 0.8

0 1.0

Figure 9.21 Schottky barrier height fn for Au/GaAsxSb1x contact, together with E0 for GaAsxSb1x (Table 6.23). The experimental data are obtained from Zhao et al. [153]. The open squares represent the endpoint binary data taken from Adachi [1]

296

PROPERTIES OF SEMICONDUCTOR ALLOYS

of E0 (Table 6.23). The solid line represents the quadratic least-squares fit given by (in eV) fn ðxÞ ¼ 0:680:88x þ 1:11x2

ð9:20Þ

We can see that both E0 and fn show a remarkable nonlinearly with respect to x.

9.2.4 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) alloy

1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

2.2 (a)

φn+φp

2.0 I-V C-V

φn+φp , E0 (eV)

φp (eV)

φn (eV)

1. GaInPAs—We show in Figure 9.22 the Schottky barrier heights fn and fp as a function of y for Au metal on GaxIn1xPyAs1y/GaAs. The sum of fn and fp, together with E0 (Table 6.28), are also plotted against y. The experimental data are taken from Lee et al. [154] and Sugino and Kousaka [155]. The Au metal on GaxIn1xPyAs1y/GaAs exhibits the SchottkyMott barrier characteristics satisfactorily (Equation (9.17)).

(b)

1.8 1.6 1.4 1.2

Au on GaxIn1-xPyAs1-x/GaAs 0

0.2

0.4

0.6

0.8

1.0

E0

1.0 0

y

(c) 0.2 0.4 0.6 0.8 1.0 y

Figure 9.22 Schottky barrier heights (a) fn and (b) fp for Au on GaxIn1xPyAs1y/GaAs. The sum fn þ fp, together with E0 (Table 6.28), are plotted against y in (c). The experimental data in (a)-(c) are taken from Lee et al. [154] and Sugino and Kousaka [155]

The Schottky barrier properties of Au metal on GaxIn1xPyAs1y/InP are shown in Figure 9.23. The fn data are taken from Morgan et al. [156] and Bhattacharya and Yeaman [157], while those for fp are from Escher et al. [158]. The solid lines represent the linear least-squares fits (in eV) fn ðxÞ ¼ 0:20 þ 0:44y

ð9:21aÞ

fp ðxÞ ¼ 0:47 þ 0:30y

ð9:21bÞ

The heavy solid line in Figure 9.23(c) shows the sum of these values against y. 2. AlGaAsSb and GaInAsSb—The Schottky barrier heights for Au, Al and Sb metals on n- and p-Al0.5Ga0.5As0.05Sb0.95/GaSb layers were studied by Polyakov et al. [159]. These authors

1.0 0.8 0.6 0.4 0.2 0 1 0.8 0.6 0.4 0.2 0

297

1.6 (a)

(c) 1.4

φn+φp , E0 (eV)

φp (eV)

φn (eV)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

(b)

0.2

0.4

0.6

0.8

1.2 1.0 E0

0.8 0.6

Au on GaxIn1-xPyAs1-y /InP 0

φn+φp

1.0

0.4 0

y

0.2 0.4 0.6 0.8 1.0 y

Figure 9.23 Schottky barrier heights (a) fn and (b) fp for Au on GaxIn1xPyAs1y/InP. The experimental data in (a) are taken from Morgan et al. [156] and Bhattacharya and Yeaman [157] and in (b) from Escher et al. [158]. The open circle is taken from Figure 9.19. The solid lines in (a) and (b) show the linear least-squares fits of Equation (9.21). The sum of fn and fp, together with E0 (Table 6.28), are plotted against y in (c)

found that the Schottky barriers are high for Au (1.3 eV) and Al (1.2 eV) on n-type material and very low on p-type materials. The behavior of Sb was unique with fn,p being 0.6–0.7 eV. The reason for the surface location of the Fermi-level pinning due to Au and Al metals may be related to a predominance of Ga-antisite-type native acceptors at the surface, which is not the case for Sb metal. The Schottky barriers for Al, Au and Sb metals on n-GaxIn1xAsySb1y/GaSb (x ¼ 0.85) were determined by Polyakov et al. [160]. All these Schottky barriers had heights of 0.5 eV, with the surface Fermi level located at Ev þ 0.16 eV. (b) (III, III, III)V alloy 1. AlGaInN—Figure 9.24 plots the fn versus x for Pd/AlxGa0.98xIn0.02N contact obtained from I V and C V measurements [161]. The alloy samples were grown on (0001)sapphire substrates by MOCVD. It was found that the larger difference in fn between IV 2.4 Pd/AlxGa0.98-xIn0.02N

φn (eV)

2.1 1.8

I-V C-V

1.5 1.2 0.9 0.6

0

0.1

0.2

0.3

x

Figure 9.24 Schottky barrier height fn for Pd/AlxGa0.98xIn0.02N contact obtained by Liu et al. [161]

PROPERTIES OF SEMICONDUCTOR ALLOYS 1.5 1.2 0.9 0.6 0.3 0 1.5 1.2 0.9 0.6 0.3 0

3.0 2.7 2.4

φn+φp , Eg (eV)

φp (eV)

φn (eV)

298

(a)

(b)

2.1

E0

1.8 1.5 1.2 0.9

φn+φp

0.6 Au on (AlxGa1-x)0.53In0.47P/GaAs

0

0.2

0.4

0.6

0.8

0.3 0 0

1.0

EgX

x

(c) 0.2 0.4 0.6 0.8 1.0 x

Figure 9.25 Schottky barrier heights (a) fn and (b) fp for Au on (AlxGa1x)0.53In0.47P/GaAs. The sum of fn and fp, together with E0 and EgX (Table 6.28), are plotted against x in (c). The experimental data are taken from Nanda et al. [137] (solid circles) and Wang et al. [162] (open circles)

and C V measurements could not be quantitatively explained by the traditional electron transport mechanisms of the Schottky barrier rectifier, such as the tunneling effect, imageforce effect or barrier inhomogeneity theory. 2. AlGaInP—The Schottky barrier heights fn and fp for Au metal on (AlxGa1x)0.53In0.47P/ GaAs are shown in Figure 9.25. The experimental data are taken from Nanda et al. [137] (solid circles) and Wang et al. [162] (open circles). The unique feature of this rectifying contact system is that both fn and fp show no strong dependence on alloy composition. If we accept the common anion rule, no strong x dependence of fp can be expected. In Figure 9.25(c), the sum of fn and fp obtained by Nanda et al. [137], together with E0 and EgX (Table 6.28), are plotted against composition x. It is apparent that fn þ fp „ E0 (or EgX ) for this rectifying contact system. 3. AlGaInAs—The Schottky barrier height fn for Au metal on (AlxGa1x)0.48In0.52As/InP has been obtained using IV and CV measurements [163]. These results are plotted in Figure 9.26. The ideality factors determined from the forward-bias IV characteristics were 0.8 Au/(AlxGa1-x)0.48In0.52As

φn (eV)

0.6 0.4 0.2 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 9.26 Schottky barrier height fn for Au on (AlxGa1x)0.48In0.52As/InP. The experimental data are taken from Schramm et al. [163]. The data represented by the open circle is taken from Figure 9.19. The solid line shows the linear least-squares fit of Equation (9.22)

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

299

in the range 1.08 1.2, indicating that the Schottky contacts were of high quality. The open circle represents the Au/Ga0.47In0.53As barrier height taken from Figure 9.19. The solid line shows the linear least-squares fit of these data (in eV) fn ðxÞ ¼ 0:20 þ 0:37x

ð9:22Þ

9.2.5 II–VI Semiconductor Alloy (a) (II, II)Te ternary alloy The Schottky barrier height fp for In metal on MgxZn1xTe determined by CV and photoelectron measurements [164] is plotted in Figure 9.27(a). The solid line shows the linear least-squares fit of these data (solid circles). This fit predicts a negative fp value of 0.36 eV (Ohmic contact) for x ¼ 1.0 (MgTe). The open circle also represents the In/pZnTe data in Adachi [165]. The dashed line corresponds to the common anion rule, fp ¼ 1.06 eV. Using this fp value and assuming ideal Schottky–Mott contact, we can estimate fn 1.4 and 1.2 eV for In/n-MgTe and In/n-ZnTe contacts, respectively. 3.6

3.0

(a) In/Mgx Zn1-xTe

(b) Au/Zn xCd1-xTe 2.4

2.4

E0

EgX

1.8 φp

1.2

Common anion rule

φp, E0 (eV)

φp, Eg (eV)

3.0

E0

1.8 1.2

φp

0.6

0.6

Common anion rule

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 9.27 (a) Schottky barrier height fp for In/MgxZn1xTe contact, together with E0 and EgX (Figure 6.58). The experimental data are taken from Akkad et al. [164]. The solid line shows the linear least-squares fit. The open circle represents the In/ZnTe data taken from Adachi [165]. The dashed line indicates the common anion rule (fp ¼ 1.06 eV). (b) Schottky barrier height fp for Au/ZnxCd1xTe contact (see text), together with E0 for ZnxCd1xTe (Table 6.30). The open circles show the Au/ZnTe and Au/CdTe data [1, 165]. The dashed line indicates the common anion rule (fp ¼ 0.6 eV)

The Schottky barrier height fp for Au metal on ZnxCd1xTe is plotted against x in Figure 9.27(b). The experimental data are taken from various sources [166–168]. These data scatter largely and fall within fp ¼ 1.0 0.4 eV (0 < x < 0.2). The open circles also show the Au/p-ZnTe and Au/p-CdTe data in Adachi [1, 165]. Using the common anion rule (fp ¼ 0.6 eV, dashed line) and assuming ideal Schottky–Mott contact, we obtain fn 1.7 and 0.9 eV for Au/n-ZnTe and Au/n-CdTe contacts, respectively. The fn value reported for Au/n-CdTe in the literature is 0.59–1.0 eV [1, 165]. No fn value has been reported for any metal/n-ZnTe contact.

300

PROPERTIES OF SEMICONDUCTOR ALLOYS

(b) Zn(VI, VI) ternary alloy ZnSxSe1x can be grown lattice-matched to GaAs (x ¼ 0.06–0.07). The Schottky contacts were formed on n-ZnS0.07Se0.93 epilayers grown on n-GaAs by MBE for metals with different work functions, Yb, Al, Cr, Cu, Au and Pd [169]. The fn value for Au/n-ZnS0.07Se0.93 contact has been plotted in Figure 9.28. The open circles represent the Au/n-ZnS and Au/n-ZnSe data taken from Adachi [1, 165]. The solid line also shows the linearly interpolated result between the endpoint binary data (in eV) fn ðxÞ ¼ 1:45 þ 0:65x

ð9:23Þ

4.2

φn, E0 (eV)

3.6

E0

3.0 2.4

φn

1.8 1.2

Au/ZnSxSe1-x

0.6 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 9.28 Schottky barrier height fn for Au/ZnSxSe1x contact, together with E0 for ZnSxSe1x (Table 6.30). The experimental data (x ¼ 0.07) is taken from Wang et al. [169]. The open circles show the Au/ZnS and Au/ZnSe data taken from Adachi [1, 165]. The solid line indicates the linearly interpolated result given by Equation (9.23)

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] K. Brunner, K. Eberl, and W. Winter, Phys. Rev. Lett. 76, 303 (1996). [3] A. A. Demkov and O. F. Sankey, Phys. Rev. B 48, 2207 (1993). [4] D. C. Houghton, G. C. Aers, N. L. Rowell, K. Brunner, W. Winter, K. Eberl, Phys. Rev. Lett. 78, 2441 (1997). [5] R. L. Williams, G. C. Aers, N. L. Rowell, K. Brunner, W. Winter, and K. Eberl, Appl. Phys. Lett. 72, 1320 (1998). [6] S. H. Ke, T. Uda, and K. Terakura, Phys. Rev. B 59, 15013 (1999). [7] G. N. Northrop, J. F. Morar, D. J. Wolford, and J. A. Bradley, J. Vac. Sci. Technol. B 10, 2018 (1992). [8] S. Fukatsu and Y. Shiraki, Appl. Phys. Lett. 63, 2378 (1993). [9] M. Wachter, K. Thonke, and R. Sauer, Thin Solid Films 222, 10 (1992). [10] T. Bajer, U. Mantz, K. Thonke, R. Sauer, F. Sch€affler, H. -J. Herzog, Phys. Rev. B 50, 15191 (1994). [11] M. L. W. Thewalt, D. A. Harrison, C. F. Reinhart, J. A. Wolk, and H. Lafontaine, Phys. Rev. Lett. 79, 269 (1997). [12] H. H. Cheng, S. T. Yen, and R. J. Nicholas, Phys. Rev. B 62, 4638 (2000). [13] B. L. Stein, E. T. Yu, E. T. Croke, A. T. Hunter, T. Laursen, A. E. Bair, J. W. Mayer, and C. C. Ahn, Appl. Phys. Lett. 70, 3413 (1997).

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

301

[14] B. L. Stein, E. T. Yu, E. T. Croke, A. T. Hunter, T. Laursen, J. W. Mayer, and C. C. Ahn, J. Vac. Sci. Technol. B 16, 1639 (1998). [15] R. Hartmann, U. Gennser, H. Sigg, D. Gr€utzmacher, and K. Ensslin, Appl. Phys. Lett. 73, 1257 (1998). [16] J. Kolodzey, F. Chen, B. A. Orner, D. Guerin, and S. I. Shah, Thin Solid Films 302, 201 (1997). [17] Y. Zhang, A. Mascarenhas, and L.-W. Wang, Appl. Phys. Lett. 80, 3111, (2002), and references cited therein. [18] D. Patel, M. J. Hafich, G. Y. Robinson, and C. S. Menoni, Phys. Rev. B 48, 18031 (1993). [19] M. D. Dawson, S. P. Najda, A. H. Kean, G. Duggan, D. J. Mowbray, O. P. Kowalski, M. S. Skolnick, and M. Hopkinson, Phys. Rev. B 50, 11190 (1994). [20] I.-J. Kim, Y.-H. Cho, K.-S. Kim, B.-D. Choe, and H. Lim, Appl. Phys. Lett. 68, 3488 (1996). [21] R. Dingle, W. Wiegmann, and C. H. Henry, Phys. Rev. Lett. 33, 827 (1974). [22] R. Dingle, A. C. Gossard, and W. Wiegmann, Phys. Rev. Lett. 34, 1327 (1975). [23] R. C. Miller, A. C. Gossard, D. A. Kleinman, and O. Munteanu, Phys. Rev. B 29, 3740 (1984). [24] R. C. Miller, D. A. Kleinman, and A. C. Gossard, Phys. Rev. B 29, 7085 (1984). [25] G. Duggan, H. I. Ralph, and K. J. Moore, Phys. Rev. B 32, 8395 (1985). [26] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, (1994). [27] S. Adachi, in Properties of Lattice-matched and Strained Indium Gallium Arsenide, EMIS Datareviews Series No. 8 (edited by P. Bhattacharya), INSPEC, London, 1993, p. 84. [28] J. B€ohrer, A. Krost, T. Wolf, and D. Bimberg, Phys. Rev. B 47, 6439 (1993). [29] E. Lugagne-Delpon, J. P. Andre, and P. Voisin, Solid State Commun. 86, 1 (1993). [30] W. Seidel, O. Krebs, P. Voisin, J. C. Harmand, F. Aristone, and J. F. Palmier, Phys. Rev. B 55, 2274 (1997). [31] J. P. Landesman, J. C. Garcia, J. Massies, P. Maurel, G. Jezequel, J. P. Hirtz, and P. Alnot, Appl. Phys. Lett. 60, 1241 (1992). [32] J. M. Lopez-Villegas P. Roura, J. Bosch, J. R. Morante, A. Georgakilas, and K. Zekentes, J. Electrochem. Soc. 140, 1492 (1993). [33] J.-H. Huang and T. Y. Chang, J. Appl. Phys. 76, 2893 (1994). [34] K. Tanaka, N. Kotera, and H. Nakamura, J. Appl. Phys. 85, 4071 (1999). [35] A. K. Srivastava, J. L. Zyskind, R. M. Lum, B. V. Dutt, and J. K. Klingert, Appl. Phys. Lett. 49, 41 (1986). [36] M. Mebarki, A. Kadri, and H. Mani, Solid State Commun. 72, 795 (1989). [37] S. S. Kizhaev, S. S. Molchanov, N. V. Zotova, E. A. Grebenshchikova, Y. P. Yakovlev, E. Hulicius, T. simecek, K. Melichar, and J. Pangrac, Tech. Phys. Lett. 27, 964 (2001). [38] H. A. Kaci, D. Boukredimi, and M. Mebarki, Phys. Status Solidi A 163, 101 (1997). [39] O. Ostinelli, G. Almuneau, and W. B€achtold, Semicond. Sci. Technol. 21, 681 (2006). [40] J. S. Nelson, S. R. Kurtz, L. R. Dawson, and J. A. Lott, Appl. Phys. Lett. 57, 578 (1990). [41] M. P. Mikhailova and A. N. Titkov, Semicond. Sci. Technol. 9, 1279 (1994). [42] M. A. Afrailov, A. N. Baranov, A. P. Dmitriev, M. P. Mikhailova, Y. P. Smorchkova, I. N. Timchenko, V. V. Sherstnev, Y. P. Yakovlev, and I. N. Yassievich, Sov. Phys. Semicond. 24, 876 (1990). [43] M. Mebarki, D. Boukredimi, and S. Sadik, J. L. Lazzari, J. Appl. Phys. 73, 2360 (1993). [44] J. R. Chang, Y. K. Su, and Y. T. Lu, J. Appl. Phys. 86, 6908 (1999). [45] M. P. Mikhailova, K. D. Moiseev, T. I. Voronina, T. S. Lagunova, and Y. P. Yakovlev, Semicond. 41, 161 (2007). [46] W. Z. Shen, S. C. Shen, W. G. Tang, Y. Chang, Y. Zhao, and A. Z. Li, J. Phys.: Condens. Matter 8, 4751 (1996). [47] J. R. Chang, Y. K. Su, C. L. Lin, K. M. Wu, W. C. Huang, Y. T. Lu, D. H. Jaw, and W. L. Li, S. M. Chen, Appl. Phys. Lett. 75, 238 (1999). [48] Y. Ishitani, E. Nomoto, T. Tanaka, and S. Minagawa, J. Appl. Phys. 81, 1763 (1997).

302

PROPERTIES OF SEMICONDUCTOR ALLOYS

[49] C. T. H. F. Liedenbaum, A. Valster, A. L. G. J. Severens, G. W. ‘t Hooft, Appl. Phys. Lett. 57, 2698 (1990). [50] O. P. Kowalski, J. W. Cockburn, D. M. Mowbray, M. S. Skolnick, R. Teissier, and M. Hopkinson, Appl. Phys. Lett. 66, 619 (1995). [51] H. K. Yow, P. A. Houston, and M. Hopkinson, Appl. Phys. Lett. 66, 2852 (1995). [52] A. D. Prins, J. L. Sly, A. T. Meney, D. J. Dunstan, Oreilly E. P. A. R. Adams, and A. Valster, J. Phys. Chem. Solids 56, 423 (1995). [53] T. M. Ritter, B. A. Weinstein, R. E. Viturro, and D. P. Bour, Phys. Status Solidi B 211, 869 (1999). [54] M. D. Dawson, G. Duggan, and D. J. Arent, Phys. Rev. B 51, 17660 (1995). [55] D. Vignaud and F. Mollot, J. Appl. Phys. 93, 384 (2003). [56] J. Shao, A. D€ornen, R. Winterhoff, and F. Scholz, Phys. Rev. B 66, 035109 (2002). [57] Y. Sugiyama, T. Inata, T. Fujii, Y. Nakata, S. Muto, and S. Hiyamizu, Jpn. J. Appl. Phys. 25, L648 (1986). [58] A. Sandhu, Y. Nakata, S. Sasa, K. Kodama, and S. Hiyamizu, Jpn. J. Appl. Phys. 26, 1709 (1987). [59] G. Martin, S. Strite, A. Botchkarev, A. Agarwal, A. Rockett, H. Morkoc, W. R. L. Lambrecht, and B. Segall, Appl. Phys. Lett. 65, 610 (1994). [60] J. Baur, K. Maier, M. Kunzer, U. Kaufmann, and J. Schneider, Appl. Phys. Lett. 65, 2211 (1994). [61] J. R. Waldrop and R. W. Grant, Appl. Phys. Lett. 68, 2879 (1996). [62] K. B. Nam, J. Li, K. H. Kim, J. Y. Lin, and H. X. Jiang, Appl. Phys. Lett. 78, 3690 (2001). [63] D. R. Hang, C. H. Chen, Y. F. Chen, H. X. Jiang, and J. Y. Lin, J. Appl. Phys. 90, 1887 (2001). [64] C. T. Foxon, S. V. Novikov, L. X. Zhao, and I. Harrison, Appl. Phys. Lett. 83, 1166 (2003). [65] A. N. Westmeyer, S. Mahajan, K. K. Bajaj, J. Y. Lin, H. X. Jiang, D. D. Koleske, and R. T. Senger, J. Appl. Phys. 99, 013705 (2006). [66] S. W. King, C. Ronning, R. F. Davis, M. C. Benjamin, and R. J. Nemanich, J. Appl. Phys. 84, 2086 (1998). [67] F. Bernardini, and V. Fiorentini, Phys. Rev. B 57, R9427 (1998). [68] C. -L. Wu, C. -H. Shen, and S. Gwo, Appl. Phys. Lett. 88, 032105 (2006). [69] P. D. C. King, T. D. Veal, P. H. Hefferson, C. F. McConville, T. Wang, P. J. Parbrook, H. Lu, and W. J. Schaff, Appl. Phys. Lett. 90, 132105 (2007). [70] C. Manz, M. Kunzer, H. Obloh, A. Ramakrishnan, and U. Kaufmann, Appl. Phys. Lett. 74, 3993 (1999). [71] H. Zhang, E. J. Miller, E. T. Yu, C. Poblenz, and J. S. Speck, Appl. Phys. Lett. 84, 4644 (2004). [72] C. -F. Shin, N. -C. Chen, P. -H. Chang, and K. -S. Liu, Jpn. J. Appl. Phys. 44, 7892 (2005). [73] T. Ohashi, P. Holmstr€om, A. Kikuchi, and K. Kishino, Appl. Phys. Lett. 89, 041907 (2006). [74] Z. H. Mahmood, A. P. Shah, A. Kadir, M. R. Gokhale, S. Ghosh, A. Bhattacharya, and B. M. Arora, Appl. Phys. Lett. 91, 152108 (2007). [75] S. P. Kowalczyk, W. J. Schaffer, E. A. Kraut, and R. W. Grant, J. Vac. Sci. Technol. 20, 705 (1992). [76] V. D. Kulakovskii, T. G. Andersson, and L. V. Butov, Semicond. Sci. Technol. 8, 477 (1993). [77] W. S. Chi, and Y. S. Huang, Semicond. Sci. Technol. 10, 127 (1995). [78] L. Lu, J. Wang, Y. Wang, W. Ge, G. Yang, and Z. Wang, J. Appl. Phys. 83, 2093 (1998). [79] Y. Zhang, A. Mascarenhas, H. P. Xin, and C. W. Tu, Phys. Rev. B 61, 7479 (2000). [80] I. A. Buyanova, G. Pozina, P. N. Hai, W. M. Chen, H. P. Xin, and C. W. Tu, Phys. Rev. B 63, 033303 (2000). [81] P. Krispin, S. G. Spruytte, J. S. Harris, and K. H. Ploog, J. Appl. Phys. 90, 2405 (2001). [82] S. Tomic, E. P. OReilly P. J. Klar, H. Gr€uning, W. Heimbrodt, W. M. Chen, and I. A. Buyanova, Phys. Rev. B 69, 245305 (2004). [83] R. Kudrawiec, M. Motyka, M. Gladysiewicz, J. Misiewicz, J. A. Gupta, and G. C. Aers, Solid State Commun. 138, 365 (2006). [84] T. Kitatani, M. Kondow, T. Kikawa, Y. Yazawa, M. Okai, and K. Uomi, Jpn. J. Appl. Phys. 38, 5003 (1999).

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT

303

[85] M. Hetterich, M. D. Dawson, A. Y. Egorov, D. Bernklau, and H. Riechert, Appl. Phys. Lett. 76, 1030 (2000). [86] G. Dumitras, and H. Riechert, J. Appl. Phys. 94, 3955 (2003). [87] J. C. Harmand, A. Caliman, E. V. K. Rao, L. Largeau, J. Ramos, R. Teissier, L. Travers, G. Ungaro, B. Theys, and I. F. L. Dias, Semicond. Sci. Technol. 17, 778 (2002). [88] F. Bousbih, S. B. Bouzid, R. Chtourou, F. F. Charfi, J. C. Harmand, and G. Ungaro, Mater. Sci. Eng. C 21, 251 (2002). [89] S. A. Lourenco, I. F. L. Dias, L. C. Poc as, J. L. Duarte, J. B. B. de Oliveira, and J. C. Harmand, J. Appl. Phys. 93, 4475 (2003). [90] R. Kudrawiec, K. Ryczko, J. Misiewicz, H. B. Yuen, S. R. Bank, M. A. Wistey, H. P. Bae, and J. S. Harris, Jr., Appl. Phys. Lett. 86, 141908 (2005). [91] G. V. Rao, F. S€auberlich, and A. Klein, Appl. Phys. Lett. 87, 032101 (2005). [92] J -J. Chen, F. Ren, Y. Li, D. P. Norton, S. J., Pearton, A. Osinsky, J. W. Dong, P. P. Chow, and J. F. Weaver, Appl. Phys. Lett. 87, 192106 (2005). [93] T. Yokogawa, T. Ishikawa, J. L. Merz, and T. Taguchi, J. Appl. Phys. 75, 2189 (1994). [94] M. Kim, C. S. Kim, S. Lee, J. K. Furdyna, and M. Dobrowolska, J. Cryst. Growth 214/215, 325 (2000). [95] M. W€ort, E. Griebl, T. Reisinger, R. Flierl, B. Haserer, T. Semmler, T. Frey, W. Gebhardt, Phys. Status Solidi B 202, 805 (1997). [96] P. M. Young, E. Runge, M. Ziegler, and H. Ehrenreich, Phys. Rev. B 49, 7424 (1994). [97] F. Liaci, P. Bigenwald, O. Briot, B. Gil, N. Briot, T. Cloitre, and R. L. Aulombard, Phys. Rev. B 51, 4699 (1995). [98] V. Pellegrini, A. Tredicucci, F. Beltram, L. Vanzetti, M. Lazzarino, and A. Franciosi, J. Appl. Phys. 79, 929 (1996). [99] C. Guenaud, E. Deleporte, A. Filoramo, P. Lelong, C. Delalande, C. Morhain, E. Tournie, and J. P. Faurie, J. Appl. Phys. 87, 1863 (2000). [100] V. I. Kozlovsky, Y. G. Sadofyev, and V. G. Litvinov, Nanotechnol. 11, 241 (2000). [101] M. W. Wang, J. F. Swenberg, M. C. Phillips, E. T. Yu, J. O. McCaldin, R. W. Grant, and T. C. McGill, Appl. Phys. Lett. 64, 3455 (1994). [102] H. Mariette, F. Dalbo N. Magnea, G. Lentz, and H. Tuffigo, Phys. Rev. B 38, 12443 (1988). [103] J. Allegre, J. Calatayud, B. Gil, H. Mathieu, H. Tuffigo, G. Lentz, N. Magnea, and H. Mariette, Phys. Rev. B 41, 8195 (1990). [104] E. Deleporte, J. M. Berroir, C. Delalande, N. Magnea, H. Mariette, J. Allegre, and J. Calatayud, Phys. Rev. B 45, 6305 (1992). [105] J. Calatayud, J. Allegre, H. Mathieu, N. Magnea, and H. Mariette, Phys. Rev. B 47, 9684 (1993). [106] V. I. Kozlovsky, Y. G. Sadofyev, and V. G. LItvinov, J. Cryst. Growth 214/215, 983 (2000). [107] von Truchseb M. V. Latussek, F. Goschenhofer, C. R. Becker, G. Landwehr, E. Batke, R. Sizmann, and P. Helgesen, Phys. Rev. B 51, 17618 (1995). [108] A. Qteish, and R. J. Needs, J. Phys.: Condens. Matter 3, 617 (1991). [109] P. M. Young, and E. Ehrenreich, Phys. Rev. B 43, 12057 (1991). [110] R. Sizmann, P. Helgesen, T. Colin, T. Skauli, and S. Lfvold, Appl. Phys. Lett. 64, 881 (1994). [111] Z. Yang, Z. Yu, Y. Lansari, S. Hwang, J. W. Cook, Jr., and J. F. Schetzina, Phys. Rev. B 49, 8096 (1994). [112] von Truchseb M. V. Latussek, C. R. Becker, and E. Batke, J. Cryst. Growth 159, 1128 (1996). [113] D. Eich, K. Ortner, U. Groh, Z. H. Chen, C. R. Becker, G. Landwehr, R. Fink, and E. Umbach, Phys. Status Solidi A 173, 261 (1999). [114] C. R. Becker, V. Latussek, Pfeuffer-Jeschke A. G. Landwehr, and L. W. Molenkamp, Phys. Rev. B 62, 10353 (2000). [115] K. Shahzad, D. J. Olego, C. G. Van de Walle, Phys. Rev. B 38, 1417 (1988). [116] M. Lomascolo, G. H. Li, K. Syassen, R. Cingolani, and I. Suemune, Phys. Rev. B 50, 14635 (1994). [117] S. Li, and J. B. Khurgin, Appl. Phys. Lett. 60, 1969 (1992).

304 [118] [119] [120] [121] [122] [123] [124] [125] [126] [127] [128] [129] [130] [131] [132] [133] [134] [135] [136] [137] [138] [139] [140] [141] [142] [143] [144] [145] [146] [147] [148] [149] [150] [151] [152] [153] [154]

PROPERTIES OF SEMICONDUCTOR ALLOYS S. Li, and J. B. Khurgin, Appl. Phys. Lett. 61, 1694 (1992). E. Pelucchi, S. Rubini, B. Bonanni, A. Franciosi, and M. Peressi, Appl. Phys. Lett. 78, 1574 (2001). Y. Wu, K. Ichino, Y. Kawakami, S. Fuijita, and S. Fujita, Jpn. J. Appl. Phys. 31, 1737 (1992). K. Kondo, H. Okuyama, and A. Ishibashi, Appl. Phys. Lett. 64, 3434 (1994). J. Suda, Y. Kawakami, S. Fujita, and S. Fujita, Jpn. J. Appl. Phys. 33, L986 (1994). T. Miyajima, F. P. Logue, J. F. Donegan, J. Hegarty, H. Okuyama, A. Ishibashi, and Y. Mori, Appl. Phys. Lett. 66, 180 (1995). K. Shahzad, J. Petruzzello, J. M. Gaines, and C. Ponzoni, Appl. Phys. Lett. 67, 659 (1995). H. Hamadeh, M. L€unenb€urger, H. Kalisch, and M. Heuken, J. Cryst. Growth 184/185, 867 (1998). H. P. Wagner, M. K€uhnelt, H. Wenisch, and D. Hommel, Phys. Rev. B 63, 235319 (2001). P. F. Baude, M. A. Haase, G. M. Haugen, K. K. Law, T. J. Miller, K. Smekalin, J. Phillips, and P. Bhattacharya, Appl. Phys. Lett. 68, 3591 (1996). K. Godo, H. Makino, M. W. Cho, J. H. Chang, S. K. Hong, T. Yao, M. Y. Shen, and T. Goto, J. Appl. Phys. 91, 5811 (2002). M. Mun~oz, H. Lu, X. Zhou, M. C. Tamargo, and F. H. Pollak, Appl. Phys. Lett. 83, 1995 (2003). Aubry-Fortuna V. M. Barthula, G. Trembiay, F. Meyer, P. Warren, and K. Lyutovitch, J. Appl. Phys. 89, 5533, (2001), and references cited therein. M. R. H. Khan, H. Nakayama, T. Detschprohm, K. Hiramatsu, and N. Sawaki, Jpn. J. Appl. Phys. 34, 6375 (1995). S. Arulkumaran, T. Egawa, G-Y. Zhao, H. Isikawa, T. Jimbo, and M. Umeno, Jpn. J. Appl. Phys. 39, L351 (2000). D. Qiao, L. S. Yu, S. S. Lau, J. M. Redwing, J. Y. Lin, and H. X. Jiang, J. Appl. Phys. 87, 801 (2000). E. D. Readinger, B. P. Luther, S. E. Mohney, and E. L. Piner, J. Appl. Phys. 89, 7983 (2001). Y. Liu, M. Z. Kauser, P. P. Ruden, Z. Hassan, Y. C. Lee, S. S. Ng, and F. K. Yam, Appl. Phys. Lett. 88, 022109 (2006). A. P. Zhang, G. Dang, F. Ren, J. Han, A. Y. Polyakov, N. B. Smimov, A. V. Govorkov, J. M. Redwing, X. A. Cao, and S. J. Pearton, Appl. Phys. Lett. 76, 1767 (2000). A. Nanda, M. J. Hafich, T. J. Vogt, L. M. Woods, G. A. Patrizi, and G. Y. Robinson, Appl. Phys. Lett. 61, 81 (1992). E. Y. Chang, Y.-L. Lai, K.-C. Lin, and C.-Y. Chang, J. Appl. Phys. 74, 5622 (1993). S. D. Kwon, H. K. Kwon, B. -D. Choe, H. Lim, and J. Y. Lee, J. Appl. Phys. 78, 2482 (1995). J. O. McCaldin, T. C. McGill, and C. A. Mead, J. Vac. Sci. Technol. 13, 802 (1976). Y. Zhu, Y. Ishimaru, N. Takahashi, and M. Shimizu, J. Appl. Phys. 80, 1617 (1996). J. Tersoff, Phys. Rev. B 32, 6968 (1985). L. P. Sadwick, C. W. Kim, K. L. Tan, and D. C. Streit, IEEE Electron Dev Lett. 12, 626 (1991). F. Gueissaz, M. Gailhanou, R. Houdre, and M. Ilegems, Appl. Phys. Lett. 60, 1099 (1992). J.-I. Chyi, J.-L. Shieh, R.-J. Lin, J.-W. Pan, and R.-M. Lin, J. Appl. Phys. 77, 1813 (1995). S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. K. Kajiyama, Y. Mizushima, and S. Sakata, Appl. Phys. Lett. 23, 458 (1973). P. Kordos, M. Marso, R. Meyer, and H. L€uth, J. Appl. Phys. 72, 2347 (1992). C. Marinelli, L. Sorba, M. Lazzarino, D. Kumar, E. Pelucchi, B. H. M€ uller, D. Orani, S. Rubini, A. Franciosi, S. D. Franceschi, and F. Beltram, J. Vac. Sci. Techonol. B 18, 2119 (2000). R. Chin, R. A. Milano, and H. D. Law, Electron. Lett. 16, 627 (1980). W. J. Keeler, A. P. Roth, and E. Fortin, Can. J. Phys. 58, 63 (1980). S. Loualiche, A. L. Corre, S. Salaun, J. Caulet, B. Lambert, M. Gauneau, D. Lecrosnier, and B. Deveaud, Appl. Phys. Lett. 59, 423 (1991). J. H. Zhao, P. F. Tang, and J. Jeong, Solid-State Electron. 35, 21 (1992). J.-K. Lee, Y.-H. Cho, B.-D. Choe, K. S. Kim, H. I. Jeon, H. Lim, and M. Razeghi, Appl. Phys. Lett. 71, 912 (1997).

HETEROJUNCTION BAND OFFSETS AND SCHOTTKY BARRIER HEIGHT [155] [156] [157] [158] [159] [160] [161] [162] [163] [164] [165] [166] [167] [168] [169]

305

T. Sugino, and T. Kousaka, Electron. Lett. 34, 595 (1998). D. V. Morgan, J. Frey, and W. J. Devlin, J. Electrochem. Soc. 127, 1202 (1980). P. K. Bhattacharya, and M. D. Yeaman, Solid-State Electron. 24, 297 (1981). J. S. Escher, L. W. James, R. Sankaran, G. A. Antypas, R. L. Moon, and R. L. Bell, J. Vac. Sci. Technol. 13, 874 (1976). A. Y. Polyakov, M. Stam, A. G. Milnes, A. E. Bochkarev, and S. J. Pearton, J. Appl. Phys. 71, 4411 (1992). A. Y. Polyakov, A. G. Milnes, L. V. Druzhinina, and I. V. Tunitskaya, Solid-State Electron. 36, 1371 (1993). Y. Liu, H. Jiang, T. Egawa, B. Zhang, and H. Ishikawa, J. Appl. Phys. 99, 123702 (2006). Y. C. Wang, J. M. Kuo, F. Ren, J. R. Lothian, and W. E. Mayo, Solid-State Electron. 42, 1045 (1998). C. Schramm, H. G. Bach, H. K€unzel, and J. P. Praseuth, J. Electrochem. Soc. 138, 2808 (1991). F. E. Akkad, A. Felimban, and F. Sallam, J. Vac. Sci. Technol. A 5, 111 (1987). S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. Q. Li, W. Jie, L. Fu, and G. Zha, Nucl. Instrum. Methods Phys. Res. A 564, 544 (2006). G. Zha, W. Jie, D. Zeng, Y. Xu, W. Zhang, and F. Xu, Surf. Sci. 600, 2629 (2006). X. Cheng, S. Zhu, B. Zhao, Z. He, D. Gao, and J. Fang, Appl. Surf. Sci. 253, 8404 (2007). A. Z. Wang, W. A. Anderson, and M. A. Haase, J. Appl. Phys. 77, 3513 (1995).

10 Optical Properties 10.1 INTRODUCTORY REMARKS 10.1.1 Optical Dispersion Relations The complex dielectric function «ðEÞ ¼ «1 ðEÞ þ i«2 ðEÞ

ð10:1Þ

can be used to describe the optical properties of the medium at all photon energies E ¼ h¯ v [1,2]. The complex refractive index n (E) can also be given by n* ðEÞ ¼ nðEÞ þ ikðEÞ ¼ «ðEÞ1=2 ¼ ½«1 ðEÞ þ i«2 ðEÞ1=2

ð10:2Þ

where n(E) is the ordinary (real) refractive index and k(E) is the extinction coefficient. From Equation (10.2), we obtain «1 ðEÞ ¼ nðEÞ2 kðEÞ2

ð10:3aÞ

«2 ðEÞ ¼ 2nðEÞkðEÞ

ð10:3bÞ

and sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð«1 ðEÞ2 þ «2 ðEÞ2 Þ1=2 þ «1 ðEÞ nðEÞ ¼ 2 sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð«1 ðEÞ2 þ «2 ðEÞ2 Þ1=2 «1 ðEÞ kðEÞ ¼ 2

ð10:4Þ

ð10:5Þ

The absorption coefficient a(E) and normal-incidence reflectivity R(E) can be given by aðEÞ ¼ RðEÞ ¼

4p kðEÞ l

ð10:6Þ

ðnðEÞ1Þ2 þ kðEÞ2 ðnðEÞ þ 1Þ2 þ kðEÞ2

where l is the wavelength of light in vacuum. Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

ð10:7Þ

308

PROPERTIES OF SEMICONDUCTOR ALLOYS

10.1.2 Static and High-frequency Dielectric Constants No detailed experimental data on the static and high-frequency dielectric constants, «s and «¥, of semiconductor alloys have been reported. The simplest linear interpolation scheme for an AxB1xC alloy is «ðxÞ ¼ x«AC þ ð1xÞ«BC

ð10:8Þ

Based on the Clausius–Mossotti relationship, we can also obtain «ðxÞ1 «AC 1 «BC 1 ¼x þ ð1xÞ «ðxÞ þ 2 «AC þ 2 «BC þ 2

ð10:9Þ

It has already been shown that Equations (10.8) and (10.9) give nearly the same results [2]. Readers will find the «s and «¥ values for some non-alloyed group-IV, III–V and II–VI semiconductors in Tables 10.2 and 10.3 of Adachi [1].

10.2 GROUP-IV SEMICONDUCTOR ALLOY 10.2.1 Binary Alloy (a) CSi The n(E) dispersion in 3C-SiC, together with that for diamond and Si, in the region below the fundamental absorption edge is shown in Figure 10.1(a). The experimental data are taken

Figure 10.1 (a) n(E) spectrum for 3C-SiC, together with those for diamond (C) and Si in the region below the fundamental absorption edge at 300 K. The experimental data are taken from Adachi [3]. (b) «(E) spectra for CxSi1x at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Optical characterization of Si1-xCx/Si (0 x 0.014) semiconductor alloys by H. Lee et al., 34, L1340. Copyright (1995), Institute of Pure and Applied Physics]

OPTICAL PROPERTIES

309

from Adachi [3]. Principally, the diamond-type crystals show no reststrahlen structure. Since 3C-SiC has the zinc-blende structure, the reststrahlen peak can be clearly seen in Figure 10.1(a) at E 0.1 eV. The optical properties of CxSi1x (x 0.014) in the IR–UV region have been studied using SE [4,5]. We reproduce in Figure 10.1(b) the «(E) spectra obtained by Lee et al. [5]. We can see that increasing the C concentration decreases the E1 (3.4 eV) and E2 CP strengths (4.3 eV), as has also been observed by Kissinger et al. [4]. (b) CGe The optical properties of CxGe1x with low C concentrations have been studied in the reststrahlen [6] and interband transition regions [6–8]. The optical absorption in the fundamental absorption edge is shifted toward the higher-energy side with increasing x [6,7]. The SE «(E) spectra measured by Krishnamurthy et al. [8] showed that increasing the C concentration decreases the E1=(E1 þ D1) (2.4 eV) and E2 CP strengths (4.2 eV), in a similar manner to that observed in CxSi1x. (c) SiGe The optical properties of relaxed SixGe1x alloy have been studied by many authors [3]. The a(E) spectra in the reststrahlen region of SixGe1x are rather complex due to a number of single- and multiple-phonon bands. The absorption coefficient is weak for the whole composition range, with a peak value of 30 cm1. Figure 10.2 shows, as an example, the reststrahlen absorption spectra for SixGe1x measured by Braunstein [9]. The samples used were selected

Figure 10.2 Far-IR absorption spectra for SixGe1x at 300 K. [Reprinted with permission from R. Braunstein, Phys. Rev. 130, 879–887 (1963). Copyright (1963) American Physical Society]

310

PROPERTIES OF SEMICONDUCTOR ALLOYS

ε2

40 30

8

(a)

x=0 0.11 0.20 0.28 0.48 0.65 0.85 1.00

4 2

SixGe1-x

0 8

(b)

(d)

6

20

4 2

10 0 1

(c)

6 n

50 40 30 20 10 0 -10 -20 50

k

ε1

for homogeneity of composition and low free-carrier concentration. Nevertheless, most of the spectra for 0.22 x 0.81 showed strong background absorption due to free carriers. Bulk single crystals were used in the x from 0 to 0.2 and from 0.9 to 1.0; the intermediate compositions were coarse polycrystals. For several at% Si in Ge or vice versa, the general features of the spectra are similar to the lattice absorption spectra of the dominant constituent, except for slight changes in the positions and shapes of the bands. Aside from the Ge- and Si-like bands present in the alloy, new bands starting at 214 and 508 cm1 are formed at the Ge and Si ends of the alloy, respectively. Both of these bands grow in intensity and shift slightly with position as the Ge and Si content are increased. Braunstein [10] studied the free-hole absorption in p-SixGe1x of various compositions. He observed the intervalence-band absorption and determined some of the VB parameters of this alloy system. The optical absorption in the fundamental absorption edge of SixGe1x has been measured by Braunstein et al. [11]. The optical constants in the IR–UV region of SixGe1x have also been determined by several authors. The «(E) and n (E) spectra for SixGe1x are shown in Figure 10.3. The experimental data are taken from Adachi [3]. The temperature dependence of the optical constants for SixGe1x has also been investigated using SE [3].

2

3 4 E (eV)

5

6

0 1

2

3 4 E (eV)

5

6

Figure 10.3 Optical constants in the IR–UV region of SixGe1x at 300 K. The experimental data are taken from Adachi [3]

The «(E) spectra for strained and relaxed SixGe1x alloys have been determined using SE [12] and it was found that the built-in strain caused a modification of the spectra in the E1 CP region. Ordering in some group-IV semiconductor alloys has also been investigated and in comparison with disordered alloys no large changes in the optical response were found [13]. (d) GeSn The optical properties of GexSn1x (x < 0.2) have been studied using optical absorption [14–16] and SE [17]. The onsets of the direct/indirect optical transitions can be clearly observed in each a(E) spectrum. However, it is difficult to determine which of the onsets is due to the direct (E0) or indirect transitions (EgL) (Figure 6.10(a)). The experimental «(E) spectra for GexSn1x [17] revealed that increasing Sn concentration decreases the E1/(E1 þ D1) (2.2 eV) and E2 CP strengths (4.2 eV). For example, the «2

OPTICAL PROPERTIES

311

strength at the E2 peak decreased from «2(E2)31 (x ¼ 1.0) to 23 (x ¼ 0.82). The CP energies were also found to show strong nonlinearity with respect to x (Figure 6.10(b)).

10.2.2 Ternary Alloy The optical properties of CxSiyGe1xy have been studied by IR absorbance in the phonon absorption region [18], by optical absorption in the fundamental absorption edge [19] and by SE in the IR–UV region [20–22]. The IR absorption spectra [18] showed that the threefold-degenerate localized phonon mode of C defects in Si splits into a number of phonon modes. The a(E) spectrum in the fundamental absorption edge revealed a clear sub-gap absorption tail in an alloy of C0.01Si0.11Ge0.88 with C primarily interstitial, not substitutional [19]. The SE «(E) spectra for CxSiyGe1xy [22] suggested that the CP strengths are reduced slightly and that the absorption at energies E 3 eV is increased with increasing x. The essentially same results have also been obtained by other authors [20,21]. Aella et al. [23] carried out SE measurements on SixGeySn1xy (x 0.25, 1 x y 0.11) and determined the composition dependence of E2 from the spectral derivative analysis.

10.3 III–V SEMICONDUCTOR TERNARY ALLOY 10.3.1 (III, III)–N Alloy (a) c-(III,III)–N alloy The optical constants of c-AlN, c-GaN and c-AlxGa1xN have been determined using SE [24]. We reproduce these results in Figure 10.4. The samples used were grown on GaAs(100) or 3C-SiC(100) by MBE. The n(E) data for c-GaN measured by K€ohler et al. [25] are also shown

Figure 10.4 (a) n(E) and (b) k(E) spectra for c-AlxGa1xN at 300 K. [Reprinted with permission from Jpn. J. Appl. Phy., Optical constants of Cubic GaN, AlN, and AlGaN Alloys by T. Suzuki et al., 39, L497. Copyright (2000), Institute of Pure and Applied Physics]

312

PROPERTIES OF SEMICONDUCTOR ALLOYS

by the solid circles. The refractive indices at l ¼ 400 nm in Figure 10.4 can be written as a function of x as nðxÞ ¼ 2:610 0:880x þ 0:364x2

ð10:10Þ

The n values in c-AlxGa1xN with lower x contents are somewhat larger than those in w-AlxGa1xN, while those with higher x contents are almost equal to the w-AlxGa1xN values. IR reflectivity in c-GaxIn1xN samples (0.769 x 1.000) grown on 3C-SiC/Si(100) by MBE has been measured in the wavenumber range between 450 and 1200 cm1 [26]. SE has also been used to determine the optical constants in the IR–UV region of c-GaxIn1xN (x ¼ 0.93–1.00) grown on GaAs(100) by MBE [27]. A parametric dielectric-function model is used to analyze the experimental SE data. (b) w-AlGaN The «(E) spectra in the IR region of w-AlxGa1xN have been measured by several authors [3,28,29]. These authors demonstrated the sensitivity afforded by IR measurements in determining the optical phonon frequencies. The n(E) dispersion in the transparent region of w-AlxGa1xN has been measured by a number of authors [30–35]. Several authors obtained not only the ordinary-ray n(E) dispersion (no, c?E) but also extraordinary-ray dispersion (ne, c||E) [31,34]. We show in Figure 10.5 the no(E) and ne(E) dispersions in w-AlxGa1xN (0 x 1.0) determined using a prism coupling waveguide technique [31]. The data clearly show the natural birefringence, i.e. Dn ¼ ne no 6¼ 0; its sign is positive for all samples and all wavelengths investigated. The temperature dependence of the n(E) dispersion has also been studied by several authors [30,35]. The absolute a(E) values have been determined for w-AlxGa1xN grown on (0001)-sapphire substrates [36,37]. The a(E) spectra measured by Omnes et al. [36] showed a sharp transition for E close to the excitonic gaps (0 x 0.35); however, the saturated a(E) values above the excitonic peaks (a 2 104 cm1) were about an order of magnitude smaller than those reported by Angerer et al. [37] (0 x 1.0). High-quality w-GaN gave a saturated a value of (1 2) 105 cm1 [3].

Figure 10.5 (a) Ordinary-ray (no) and (b) extraordinary-ray refractive indices (ne) for w-AlxGa1xN at € ur, H. O. Everitt, F. Yun, and H. Morkoç, € Ozg€ 300 K. [Reprinted with permission from G. Webb-Wood, U. Phys. Status Solidi A 188, 793 (2001), Copyright (2001) Wiley–VCH]

OPTICAL PROPERTIES 15

(a)

10

x=0

10

0.11

5

5 0.23

ε2

ε1

0 -5 0.29 0.45 0.53

-10 -15

0

2

E1

E2

E3

0 -5 -10 -15

w-AlxGa1-xN

-20

(b) E0

313

4 6 E (eV)

-20 8

10

2

4

6 E (eV)

8

10

Figure 10.6 «(E) spectra for w-AlxGa1xN at 300 K. Successive spectra are vertically shifted by 4.4, 9.2, 11.6, 18.0 and 21.2, respectively. [Reprinted with permission from C. Buchheim et al., Phys. Status Solidi B 242, 2610 (2005), Copyright (2005) Wiley–VCH]

The SE «(E) spectra for w-AlxGa1xN have been measured by many authors (see e.g. [33,35,38–40]). Figure 10.6 shows the «(E) spectra obtained by Buchheim et al. [40] for samples at x ¼ 00.53. The four CPs (E0 E3) can be clearly seen in the lower x samples. As expected, these CPs undergo a continuous shift to higher energies with increasing x. However, the E3 CP shows a different behavior: it decreases with increasing x to overlap with E2 at high x contents. The origin of such an unusual shift is unclear at present. The «(E)-related optical constants have been interpreted by a simplified interband-transition model, known as the MDF [2,41]. (c) w-AlInN The optical photon behaviors in w-AlxIn1xN with the limited composition of 0.12 x 0.21 have been investigated using IR ellipsometry [42]. The n(E) dispersion in polycrystalline w-AlxIn1xN films has been determined by measuring reflectivity spectra [45]. The modeled n(E) dispersion has also been reported by Laws et al. [43]. The optical absorption spectra a(E) have been measured to determine the fundamental absorption edge in w-AlxIn1xN [44,45]. The SE «(E) spectra for w-AlxIn1xN have been measured by Goldhahn et al. [46]. These results are reproduced in Figure 10.7. The samples used were grown on (0001)-sapphire substrates. The data presented in Figure 10.7 correspond to those for the ordinary ray. The five CPs (E0 E4) can be clearly seen in the «(E) spectra. The unknown peak (A) has also been found in the lower-energy side of the E1 peak. (d) w-GaInN The reflectivity spectra R(E) in the reststrahlen region of w-GaxIn1xN have been measured by Osamura et al. [47]. The samples were polycrystallites grown by electron-beam plasma deposition. The refractive index and natural birefringence in w-GaxIn1xN (0.934 x 0.964) have been determined by a prism coupling method in conjunction with multilayer optical waveguide analysis [48] and found to show positive birefringence (Dn ¼ ne no > 0). Laws et al. [43] obtained the modeled n(E) dispersion curves with x from 0.75 to 0.95. The optical absorption spectra a(E) have also been determined by several authors [49–51].

314

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.7 «(E) spectra for w-AlxIn1xN at 300 K. Successive spectra are vertically shifted by 2.7, 5.1 and 8.7, respectively. [Reprinted with permission from R. Goldhahn et al., Phys. Status Solidi A 203, 42 (2006), Copyright (2006) Wiley–VCH]

The «(E) spectra in the visible–UV region of w-GaxIn1xN have been measured by SE [52,53] and electron energy-loss spectroscopy [54]. The SE «(E) spectra exhibited a clear maximum at the fundamental absorption edge, which allowed the determination of the Ga content x [52]. The «1(E) data in the transparent region have also been analyzed using the Sellmeier-type dispersion model [53].

10.3.2 (III, III)–P Alloy (a) AlGaP AlxGa1xP is one of the least studied III–V ternaries. The IR reflectivity has been measured [55]. The low-temperature a(E) spectra in the fundamental absorption edge of AlxGa1xP (0 x 1.0) have also been determined [56]. The n(E) values at several wavelengths for AlxGa1xP (0 x 0.3) have been measured using a phase diffraction grating method [57]. The «(E) spectra in the visible–UV region of AlxIGa1xP have been measured using SE [58,59]. The «(E) spectra obtained by Choi et al. [59] have been reproduced in Figure 10.8. The samples were grown on GaP(100) by gas-source MBE. The interference oscillations can be seen in the transparent region of the alloys. The energy at which the oscillations disappear provides an estimate of E0. The CPs, such as E0, E1 and E2, can be clearly identified in these spectra. (b) AlInP AlxIn1xP with x 0.5 can be epitaxially grown on GaAs substrate. The optical properties of AlxIn1xP are not well known, except for Al0.5In0.5P. Data on the optical constants of Al0.5In0.5P can be found as the endpoint material of the AlxGayIn1xyP/GaAs quaternary.

OPTICAL PROPERTIES

315

Figure 10.8 «(E) spectra for AlxGa1xP at 300 K. Successive spectra are offset in multiples of 10 for clarity. [Reprinted with permission from S. G. Choi et al., J. Appl. Phys. 87, 1287–1290 (2000). Copyright (2000), American Institute of Physics]

(c) GaInP The IR reflectivity in GaxIn1xP has been measured in the spectral ranges of 260–500 [60] and 220–500 cm1 [61]. Brillouin scattering has been used to determine the complex refractive indices n (E) in the region below the fundamental absorption edge of Ga0.52In0.48P latticematched to GaAs [62]. The optical absorption and hydrostatic-pressure effect at the fundamental absorption edge of GaxIn1xP (0.36 x 0.5) have also been measured by Go~ni et al. [63]. A crossover from direct to indirect fundamental gap is found to occur at p ¼ 5.0 (x ¼ 0.36) and 2.7 GPa (x ¼ 0.5) at 300 K. The optical properties of GaxIn1xP (0.494 x 0.584) grown on GaAs have been investigated using SE [64]. The optical functions of Ga0.52In0.48P lattice-matched to GaAs have also been determined using SE [65,66]. The «(E) and n (E) spectra for Ga0.52In0.48P determined by SE as an endpoint material of the AlxGayIn1xyP/GaAs quaternary [3] are shown in Figure 10.9. The effects of ordering on the optical properties of GaInP2 alloy have

25 15

ε

10 5

5

ε2

0

Ga0.52In0.48P

n

3 2 1

-5 -10

(b)

4

ε1

n, k

20

6

(a)

0 1 2 3 4 5 6 E (eV)

k

0 0 1 2 3 4 5 6 E (eV)

Figure 10.9 Optical constants in the IR–UV region of Ga0.52In0.48P/GaAs at 300 K. The experimental data are taken from Adachi [3]

316

PROPERTIES OF SEMICONDUCTOR ALLOYS

also been investigated using SE [67] and found to be relatively weak, yet significant near the fundamental absorption edge and for the higher-lying CPs.

10.3.3 (III, III)–As Alloy (a) AlGaAs The «(E) and n (E) spectra in the reststrahlen region of AlxGa1xAs (0 x 1.0) [3] have been plotted in Figure 10.10. The experimental data are taken from Adachi [3]. The two phonon bands, GaAs-like and AlAs-like, are clear and distinct in Figure 10.10. No additional structure was found in the frequency range 50–700 cm1 [3]. (a) AlAs-like

160 120 80 40 0 200

n

x 0 0.18 0.36 0.54 1.00

(b) k

ε2

ε1

160 120 GaAs-like 80 40 0 -40 -80 -120 240 200

250 300 350 Frequency (cm -1 )

400

16 14 12 10 8 6 4 2 0 16 14 12 10 8 6 4 2 0 200

(c)

AlxGa1-xAs

250 300 350 Frequency (cm -1 )

(d)

400

Figure 10.10 Optical constants in the reststrahlen region of AlxGa1xAs at 300 K. The experimental data are taken from Adachi [3]

The n(E) dispersion in the transparent region of AlxGa1xAs is shown in Figure 10.11. These curves are obtained from a method for calculating n(E) dispersion below E0 [3,68]. The composition dependence of the strength parameters is expressed as continuous functions of x. This insures that the n(E) dispersion in both optional composition x and photon energy E can be calculated, as demonstrated in Figure 10.11. Aspnes et al. [69] reported the room-temperature optical constants in the near-IR–UV region of AlxGa1xAs of target compositions x ¼ 0–0.80 in steps of 0.10 at energies between 1.5 and 6.0 eV determined by SE. The actual compositions were not different from the target compositions by more than 0.02. The accuracy of the pseudodielectric function at selected wavelengths in the technologically relevant composition range of x ¼ 0–0.5 was less than 2% of its peak value. These results are plotted in Figure 10.12. The optical properties in the far-IR–UV region of GaAs, AlAs and AlxGa1xAs published up until 1992 have been reviewed by Adachi [70]. There have been several publications since 1993. They concern a(E) in the fundamental absorption edge [71], n(E) in the terahertzE0 (Eg) region [72–77] and SE «(E) in the near-IR–UV region [78,79]. (b) AlInAs The absorption coefficients a(E) and refractive indices n(E) of AlxIn1xAs, including Al0.48In0.52As/InP, have been measured by several authors [80–84] (see n(E) in Figure 10.31).

OPTICAL PROPERTIES

317

Figure 10.11 n(E) spectra for AlxGa1xAs with increments in x of 0.1 at 300 K. [Reprinted with permission from S. Adachi, J. Appl. Phys. 58, R1–R29 (1985). Copyright (1985), American Institute of Physics]

(a) n

30 25 20 15 10 5 0 -5 -10 -15 35 30 25 20 15 10 5 0 1

x 0 0.099 0.198 0.315 0.419 0.491 0.590 0.700 0.804 1.000 2

(b) k

ε2

ε1

The optical properties in the interband transition region of AlxIn1xAs have been studied using SE by Rodrıguez and Armelles [58] (0 x 1.0), Dinges et al. [85] (x ¼ 0.48) and Kamlet and Terry [86] (0.305 x 0.635). Figure 10.13(a) shows the «(E) spectra for x ¼ 0.48 obtained by Kamlet and Terry [86]. The n (E) spectra were calculated from these «(E) spectra and are shown in the lower part of Figure 10.13(a). The E1 and E2 peaks can be clearly identified at E3 and 4.6 eV, respectively.

3 4 E (eV)

5

6

6 5 4 3 2 1 0 6 5 4 3 2 1 0 1

(c)

AlxGa1-xAs

(d)

2

3 4 E (eV)

5

6

Figure 10.12 Optical constants in the near-IR–UV region of AlxGa1xAs at 300 K. The experimental data are taken from Adachi [3]

318

PROPERTIES OF SEMICONDUCTOR ALLOYS

(a)

30 20 ε1 10 ε2 0 -10 Ga0.47In0.53As 5 4 n 3 2 k 1 0 6 1 2 3 4 E (eV)

(b)

n, k

n, k

ε

ε

30 20 ε1 10 ε 2 0 -10 Al0.48In0.52As 5 4 n 3 2 k 1 0 1 2 3 4 E (eV)

5

5

6

Figure 10.13 (a) Optical constants in the near-IR–UV region of Al0.48In0.52As/InP at 300 K. The experimental data are taken from Kamlet and Terry [86]. (b) Optical constants in the near-IR–UV region of Ga0.47In0.53As/InP at 300 K. The experimental data are taken from Adachi [3]

(c) GaInAs There have been many reports on the optical properties of GaxIn1xAs. This is especially true for Ga0.47In0.53As lattice-matched to InP [87]. More recently, some authors have carried out reflectivity measurements in the reststrahlen region of GaxIn1xAs to characterize the behavior of the long-wavelength optical phonons in strained epilayers [88–90] and also to elucidate plasma reflection [91]. The n(E) dispersion in GaxIn1xAs (0.53 x 1.00) has been determined from reflectance measurements by Takagi [92]. Note that his extrapolated x ¼ 0.47 value, n 3.43 at E ¼ 1.2 eV, is considerably smaller than that reported by Adachi [3] (n 3.6, see Figure 10.31). The optical properties in the visible–UV region of GaxIn1xAs over the entire composition range (0 x 1.0) have been studied using SE [93,94]. Figure 10.14 shows these results [93]. The peaks in «2 at 2.53 and 4.5 eV correspond to the E1/(E1 þ D1) and E2 CPs,

Figure 10.14 «(E) spectra for GaxIn1xAs at 300 K. Successive spectra are offset by 8 and 7 in (a) and (b), respectively. [Reprinted with permission from T. J. Kim et al., Phys. Rev. B 68, 115323 (2003). Copyright (2003) by the American Physical Society]

OPTICAL PROPERTIES

319

respectively. Several authors also used SE to obtain «(E) spectra for Ga0.47In0.53As/InP. The corresponding «(E)-related spectra are shown in Figure 10.13(b) [3]. A series of strained and relaxed GaxIn1xAs layers on GaAs have also been examined using SE [95–98]. Additional information relating to the critical thickness for pseudomorphic growth of GaxIn1xAs on GaAs has been derived [97].

10.3.4 (III, III)–Sb Alloy (a) AlGaSb

n

The IR optical constants of AlxGa1xSb have been determined in the spectral range of 20–520 cm1 [99–102]. The reststrahlen parameters obtained have been given in tabular form [99,101,102]. The n(E) dispersion in the 0.5–1.3 eV region of AlxGa1xSb (0 x 0.73) has been determined from reflectivity measurements by Ance and Van Mau [103]. These results and those for AlSb and GaSb presented in Adachi [3] are shown in Figure 10.15. The optical absorption spectra a(E) for AlxGa1xSb (x 0.41) have also been measured at 2 K and fitted by taking into account the excitonic effects [104]. 4.3 4.2 4.1 4.0 3.9 3.8 3.7 3.6 3.5 3.4 3.3 3.2 3.1

AlxGa1-xSb x=0 0.10 0.24 0.34 0.42 0.48

1.00

0.73

0.4

0.6

0.8 E (eV)

1.0

1.2

Figure 10.15 n(E) spectra for AlxGa1xSb at 300 K. The experimental data are taken from Adachi [3]

SE has been used to characterize epitaxial AlxGa1xSb layers for different x compositions in the 1.4–6 eV region [102,105,106]. The CP parameters and their composition dependence are determined by performing a standard CP analysis. The «(E) spectra obtained by Choi et al. [106] are reproduced in Figure 10.16. (b) GaInSb The IR reflectivity spectra of GaxIn1xSb have been measured in the range 135–285 cm1 by Brodsky et al. [107] and 100–350 cm1 by Feng et al. [108]. The reststrahlen parameters have been tabulated by Brodsky et al. [107]. The absorption spectra a(E) in the fundamental absorption edge of GaxIn1xSb have also been measured at 300 K [109]. Imai and Adachi [110] have obtained the optical constants in the 1.5–5.4 eV region of GaxIn1xSb using SE at 300 K. The samples were grown by a conventional Bridgman method. The n (E) spectra obtained by Imai and Adachi [110] are shown in Figure 10.17. These authors also determined the x-dependent CP parameters from the MDF analysis.

320

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.16 «(E) spectra for AlxGa1xSb at 300 K. Successive spectra are offset upward from the x ¼ 0.39 spectrum by multiples of 5 for clarity. [Reprinted with permission from S. G. Choi, C. J. Palmstrem, Y. D. Kim, S. L. Cooper, and D. E. Aspnes, J. Appl. Phys. 98, 104108 (2005). Copyright (2005), American Institute of Physics]

10.3.5 Dilute-nitride III–(V, V) Alloy (a) GaNP The IR reflectivity spectra of dilute-nitride GaNxP1x have been measured in the spectral ranges of 300–600 cm1 (0.006 x 0.0285) [111] and 50–4000 cm1 (0 x 0.15) [112]. These spectra led to the determination of the GaN- and GaP-like phonon frequencies. The nature of the fundamental absorption edge of GaNxP1x was elucidated using the a(E) spectra [113–115]. The experimental data obtained by Rudko et al. [113] suggest that the absorption edge of GaNxP1x with x ¼ 0.01–0.03 exhibits a direct band-gap-like behavior. The a(E) spectra obtained by Buyanova et al. [114] have been explained by the BAC model (Section 6.3.5). On the other hand, the low-temperature absorption data obtained by

Figure 10.17 n(E) and k(E) spectra for GaxIn1xSb with increments in x of 0.25 at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Optical constants of In1-xGaxSb ternary alloys: Experiment and modeling by S. Imai and S. Adachi, 32, 3860. Copyright (1993), Institute of Pure and Applied Physics]

OPTICAL PROPERTIES

321

Fluegel et al. [115] indicate that the host CB minimum near X does not plunge downward with increased N doping. These results challenge the validity of the BAC and polymorphous model for GaNxP1x, but corroborate the conclusion that due to the dissimilarity between GaNxP1x and GaNxAs1x, seeking a universal model for the band-gap lowering that applies to both the isoelectronic doping systems is unrealistic. SE has been used to investigate the electronic energy-band structure of GaNxP1x [114,116]. The «2(E) spectra obtained by Leibiger et al. [116] are reproduced in Figure 10.18. The vertical dotted lines mark the CPs, E0, E1, E00, E2 and E10, determined by MDF analysis.

Figure 10.18 «2(E) spectra for dilute-nitride GaNxP1x at 300 K. Successive spectra are offset in multiples of 4 for clarity [Reprinted with permission from G. Leibiger, V. Gottschalch, M. Schubert, G. Benndorf, and R. Schwabe, Phys. Rev. B 65, 245207 (2002). Copyright (2002) by the American Physical Society]

(b) GaNAs The absorption coefficient a(E) in the fundamental absorption edge of GaNxAs1x has been measured by several authors (see e.g. [117–119]). The a(E) spectra recorded by Tisch et al. [119] (0 x 0.05) are shown in Figure 10.19. It can be seen that for all samples a2 depends linearly on E up to 108 cm2. The slope of the linear part of a2 decreases and the Urbach tail increases with increasing N fraction. The decrease in the fundamental absorption edge (E) with increasing x can be clearly seen (see also Figure 6.29(b)). The optical properties of GaNxAs1x have been studied using SE by many authors (see e.g. [120–122]). The «(E) spectra recorded by Leibiger et al. [122] are shown in Figure 10.20. The «(E)-related spectra, «(E) and n (E), were found to agree very well with the MDF approach [120–122]. Note that the fundamental absorption edge (E) observed in Figure 10.20 follows the well-known redshift with increasing x. (c) GaNSb FTIR measurements on GaNxSb1x have been undertaken by Jefferson et al. [123]. The divergence of transitions from the VB to E and E þ has been observed with increasing N incorporation, consistent with the BAC model (Figure 6.29(c)).

322

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.19 a2 versus E plots for dilute-nitride GaNxAs1x at 300 K. [Reprinted with permission from U. Tisch, E. Finkman, and J. Salzman, Appl. Phys. Lett. 81, 463 (2002). Copyright (2002), American Institute of Physics]

(d) InNP Optical absorption measurements were carried out to investigate the N incorporation effect into InP [124]. A band-gap reduction of 0.15 eV was observed with N incorporation of 0.9 at%. (e) InNAs IR reflectivity and Hall-effect measurements have been carried out to determine the x-dependent electron effective mass in InNxAs1x [125] (Figure 7.11). The N-induced reduction of the fundamental absorption edge has also been confirmed in InNxAs1x by plotting a2 versus E [126] (Figure 6.31(b)).

10.3.6 Al–(V, V) Alloy An AlPSb layer lattice-matched to InP was grown by gas-source MBE [127]. Using an ellipsometer, the refractive index of this alloy at l ¼ 1.55 mm was determined to be 3.037.

Figure 10.20 «(E) spectra for dilute-nitride GaNxAs1x at 300 K. Successive spectra are offset upward from the x ¼ 0.10 at% spectrum by multiples of 3 for clarity. [Reprinted with permission from G. Leibiger, and M. Schubert, J. Appl. Phys. 89, 4927 (2001). Copyright (2001), V. Gottschalch, B. Rheinl€ander, J. Sik, American Institute of Physics]

OPTICAL PROPERTIES

323

Saadallah et al. [128] carried out photothermal deflection measurements on an MBE-grown AlAs0.08Sb0.92/GaSb layer and determined the n(E) and a(E) spectra, in addition to the thickness of the layer and its thermal conductivity. The Sellmeier parameters which were determined are: A ¼ 8.82, B ¼ 0.79 and C ¼ 0.589 mm (see Equation (10.71) in Adachi [1]). The fundamental absorption edge of AlAs0.08Sb0.92 was also estimated to be 1.55 eV (Figure 6.32(b)).

10.3.7 Ga–(V, V) Alloy (a) GaPAs The n(E) dispersion in GaPxAs1x has been studied by several authors [129–131]. The n(E) data obtained by Clark and Holonyak [129] and Casey [130] agree closely between 1.2 and 1.75 eV where comparison is possible. The experimental data at 87 and 300 K by Clark and Holonyak [129] were fitted to the first-order Sellmeier equation. This enables us to calculate the n(E) dispersion in a given alloy of composition x and photon energy E. These results are shown in Figure 10.21. The calculated n(E) values are taken from Adachi [3]. The resulting n(E) dispersion is found to decrease with increasing x. 3.6 3.5

n

3.4

x=0

3.3 3.2 GaPxAs1-x

3.1 3.0 0.4

x=1.0

0.8

1.2 1.6 E (eV)

2.0

2.4

Figure 10.21 n(E) dispersion in the transparent region of GaPxAs1x with increments in x of 0.1 at 300 K. The n values are taken from Adachi [3]

Clark and Holonyak [129] investigated the optical absorption spectra in the IR and fundamental absorption edge regions of GaPxAs1x. They observed the free-carrier and interconduction-band absorption in GaAs-rich alloys and donor-related absorption in GaP-rich alloys. The Burstein–Moss shift of the fundamental absorption edge was also observed. The optical absorption in GaPxAs1x (0.29 x 0.43) has also been examined by Nelson et al. [132] who observed distinct free-exciton peaks (n ¼ 1 and 2) at 4.2 K and a peak (n ¼ 1) at T 77 K. The direct-exciton binding energy G for GaPxAs1x obtained by Nelson et al. [132] is plotted in Figure 10.22 as a function of x, together with the corresponding values for GaP and GaAs taken from Adachi [1]. The direct-exciton (E0) and indirect-exciton binding energies (EgX ) for GaP are 13 and 22 meV, respectively (see Table 10.4 in Adachi [1]). The G values for GaPxAs1x in Figure 10.22 are considerably smaller than those obtained from the linear interpolation scheme. Thomson et al. [133] measured the fundamental reflectivity spectra of GaPxAs1x at 80 and 295 K. More recently, Kim et al. [134] reported the «(E) spectra of GaPxAs1x layers grown

324

PROPERTIES OF SEMICONDUCTOR ALLOYS 20 GaPxAs1-x

G (meV)

15 10 5 0

0

0.2

0.4

x

0.6

0.8

1.0

Figure 10.22 Direct-exciton binding energy G versus x for GaPxAs1x. The experimental data (solid circles) are taken from Nelson et al. [132]. The open squares show the endpoint binary data taken from Adachi [1]

by VPE on GaAs(100) (x ¼ 0.2 and 0.4) and on GaP(100) (x ¼ 0.7). The measured «(E) spectra revealed distinct structures at energies of the E0, E1, E1 þ D1, E00 and E2 CPs. (b) GaPSb GaPxSb1x lattice-matched to InP was grown by gas-source MBE [127]. Using an ellipsometer, the refractive index of this alloy at l ¼ 1.55 mm was determined to be 3.579. A highly reﬂective distributed Bragg reﬂector was demonstrated using AlPxSb1x/GaPxSb1x, which showed a stop-band width of 206 nm with maximum reflectivity exceeding 99% at l 1.6 mm. (c) GaAsSb The IR reflectivity spectra of GaAsxSb1x have been measured in the 200–320 cm1 range by Lukovsky and Chen et al. [135]. A reflectance band was observed in the x ¼ 0.85 composition, whereas at least two bands were evident in the x ¼ 0.20 and 0.25 samples. In the latter two samples, the structure near 240 cm1 was due to the phonon modes, whereas the structure at lower energies (230 cm1) was due to free-carrier plasma effects. Optical absorption measurements were undertaken on GaAsxSb1x by several authors [136–138]. The measured data were used to determine E0 [136] and its temperature dependence [137,138]. The fundamental reflectivity spectra were measured on evaporated GaAsxSb1x films on glasses and on bulk samples [139]. SE and PR were used to determine the x dependence of some CPs, such as E0, E1 and E2, in epitaxial GaAsxSb1x/GaAs(100) layers (0.44 x 1.00) [140]. More recently, Serries et al. [141] used SE and Raman scattering to investigate pseudomorphically strained GaAsxSb1x layers (0.35 x 0.78) grown on InP(100).

10.3.8 In–(V, V) Alloy (a) InPAs The reflectivity spectra in the reststrahlen region of InPxAs1x have been measured by several authors [142,143]. These studies gave similar results; however, the InP- and InAs-like

OPTICAL PROPERTIES

325

oscillator strengths determined by Lockwood et al. [143] vary considerably from those reported by Kekelidze et al. [142]. The plasma reflection characteristics have also been studied by Charache et al. [91]. The alloy composition dependence of E0 has been determined by plotting a2 versus E [144]. The «(E) spectra have also been obtained for InPxAs1x/InP(100) samples using SE [145]. The x dependence of the E1, E1 þ D1 and E2 CPs have been determined by analyzing the second-derivative spectra of «(E). The «(E) spectra obtained by Choi et al. [145] have been reproduced in Figure 10.23.

Figure 10.23 «(E) spectra for InPxAs1x at 300 K. Successive spectra are offset in multiples of 10 for clarity [Reprinted with permission from S. G. Choi, C. J. Palmstrøm, Y. D. Kim, D. E. Aspnes, H. J. Kim, and Y.-C. Chang, Appl. Phys. Lett. 91, 041917 (2007). Copyright (2007), American Institute of Physics]

(b) InPSb The optical absorption spectra a(E) have been measured to determine the x dependence of E0 for MOCVD-InPxSb1x layers [146] (Figure 6.37(a)). The spectra show long band tails, which extend further into the gap as the Sb concentration is increased. The band tails are considered to be caused by compositional clustering. (c) InAsSb The optical reflectivity in the reststrahlen region of InAsxSb1x has been studied in the 135–285 cm1 range by Lucovsky et al. [135] and in the 50–300 cm1 range by Rowell et al. [147]. Plasma-edge reflectance data obtained by Thomas and Woolley [148] suggested that «¥ for InAsxSb1x can be given by the linear interpolation between the endpoint binary data within experimental accuracy. Optical absorption and transmittance measurements have been carried out to characterize InAsxSb1x layers grown on GaAs [149,150], GaSb [151] and InAs [152]. The data are mainly used to determine E0 in these alloy layers. Note that all these substrates are transparent for light wavelengths at or below the InAsxSb1x gap (0 x 1.00). SE measurements have been undertaken for InAsxSb1x layers grown on InAs(100) [153,154]. The alloy compositions investigated were 0.89 x 0.96 [153] and 0 x 0.06 [154].

326

PROPERTIES OF SEMICONDUCTOR ALLOYS

10.4 III–V SEMICONDUCTOR QUATERNARY ALLOY 10.4.1 Dilute-nitride Quaternary Alloy (a) GaInNP The optical properties of GaxIn1xNyP1y epilayers on GaP(100) have been investigated using SE [155]. The compositions of GaxIn1xNyP1y layers were changed to satisfy the latticematching condition, i.e. x 1y, with 0 y 0.035. The SE-derived spectra, n(E), k(E) and a(E), were presented in graphical form. (b) GaInNAs Far-IR SE has been used to investigate the reststrahlen properties of GaxIn1xNyAs1y (x > 0.87, y < 0.03) [156]. The plasma reflection spectra have also been measured to determine the CB dispersion relationships in GaxIn1xNyAs1y [157]. This study also reported the temperature- and pressure-dependent optical absorption at the fundamental absorption edge of free-standing GaxIn1xNyAs1y layers (0.91 x 1.00, 0 y 0.025) lattice-matched to GaAs. The n(E) dispersion in the transparent region of strained GaxIn1xNyAs1y layers has been measured by several authors [156,158]. The SE-derived n(E) and k(E) spectra were analyzed using the MDF approach [156]. The SE «(E) spectra in the interband transition region of GaxIn1xNyAs1y have also been reported by Skierbiszewski [157]. These results have been reproduced in Figure 10.24. It can be seen that the N incorporation has a large effect on the optical dispersion relationships in the E1/(E1 þ D1) transition region (3 eV).

Figure 10.24 «(E) spectra for dilute-nitride GaxIn1xNyAs1y at 300 K. Successive spectra are offset in multiples of 5 for clarity [Reprinted with permission from C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002), Copyright (2002) Institute of Physics]

10.4.2 (III, III)–(V, V) Alloy (a) AlGaPAs The IR reflectivity spectra in the 200–500 cm1 range of AlxGa1xPyAs1y have been measured by Sen and Lucovsky [159]. The reststrahlen parameters obtained were reported in tabular form. The optical absorption spectra a(E) at the fundamental absorption edge of

OPTICAL PROPERTIES

327

AlxGa1xPyAs1y have also been measured by Kuznetsov et al. [160]. The single-crystalline alloys used were grown on GaP by LPE with several pairs of composition (x, y). (b) AlGaAsSb The IR reflectivity spectra in the range of 75–400 cm1 for AlxGa1xAsySb1y/GaSb have been measured by Mezerreg et al. [161]. The reststrahlen parameters obtained were presented in tabular form. Alibert et al. [162] obtained the n(E) dispersion in LPE-grown AlxGa1xAsySb1y/GaSb layers. The n(E) data were determined from accurate measurement of the p-polarized light reflection as a function of the incident angle. The data in the limit E ! 0 eV (i.e. «¥ values) showed very strong nonlinearity with respect to x [162]. The n(E) data for AlxGa1xAsySb1y/ InP (x ¼ 0.1) have also been determined from reflectance measurements [163]. The n(E) dispersion in AlxGa1xAsySb1y/InP obtained from the MDF calculation [2] is shown in Figure 10.25. The solid circles represent the experimental data taken from Blum et al. [163].

Figure 10.25 n(E) dispersion in the transparent region of AlxGa1xAsySb1y/InP with increments in x of 0.1 at 300 K, together with that for InP. The n(E) curves are calculated from the simplified interbandtransition model [2]. The experimental data by Blum et al. [163] are represented by the solid circles (x ¼ 0.1)

The absorption coefficients for LPE-grown AlxGa1xAsySb1y layers on GaAs with (x, y) ¼ (0, 0.9) and (0.06, 0.9) have been determined at several temperatures between 20 and 300 K [164]. Note that this material system is not a lattice-matched system. (c) GaInPAs The IR reflectivity spectra of GaxIn1xPyAs1y/InP have been measured by several authors [3]. The optical constants in the reststrahlen region can be usually determined by using KramersKr€ onig transformation or from the fit to an oscillator model. However, no detailed reststrahlen parameters have been determined for GaxIn1xPyAs1y/InP. This is because many IR studies were focused on multi-phonon behaviors (Section 4.2).

328

PROPERTIES OF SEMICONDUCTOR ALLOYS

The n(E) measurements in the transparent region were carried out using various techniques [3]. Accurate experimental data relating to the optional composition of GaxIn1xPyAs1y are, however, not yet available. Thus, some type of calculation is necessary. Different approaches have been used to calculate the n(E) dispersion. Our calculated n(E) curves for InxGa1xAsyP1y=InP based on the simplified interband-transition model [2] are presented in Figure 10.26.

Figure 10.26 n(E) dispersion in the transparent region of GaxIn1xPyAs1y/InP with increments in y of 0.1 at 300 K. The n(E) curves are calculated from the simplified interband-transition model [2]

Near-band-edge absorption in GaxIn1xPyAs1y/InP has been studied by many investigators [3]. The spectra depicted the sharp decline of a, common to the direct-band-gap semiconductors. Since the experimental information seemed to be limited to narrow composition and wavelength ranges, Fiedler and Schlachetzki [165] calculated the absorption coefficients for GaxIn1xPyAs1y using the extrapolation scheme. The optical constants in the interband transition region of GaxIn1xPyAs1y/InP have been studied using SE [3]. Kelso et al. [166] reported the room-temperature optical constants for GaxIn1xPyAs1y/InP of target compositions y ¼ 0–1.0 in steps of 0.2 at energies E ¼ 1.5–6.0 eV measured by SE. The samples were grown by LPE with carrier concentrations in the 1016–1017 cm3 range. The complex optical constants, «(E) and n (E), obtained from this study [3,166] are shown in Figure 10.27. The n(E) data in the transparent region (l ¼ 808, 850 and 980 nm) of GaxIn1xPyAs1y/ GaAs have been determined using variable-angle SE [167]. As expected, the n value decreased with increasing E0, i.e. increasing y (Figure 6.44(a)). (d) GaInAsSb The IR reflectivity spectra for GaxIn1xAsySb1y/GaSb epilayers have been measured by Mezerreg et al. [161] and Pickering [168]. The reststrahlen parameters obtained were presented in tabular form [161]. Studies on GaxIn1xAsySb1y/InAs have also been undertaken by Pickering [168]. Bi et al. [169] reported the IR absorption properties of MBE-grown GaxIn1xAsySb1y layers on GaAs and GaSb substrates. They also obtained n(E) curves in the 600–3200 cm1 range

25 20 15 10 5 0 -5 -10 25

5

(a)

4 3 2

y=0 0.18 0.45 0.58 0.76 1.00

1

(b)

(c)

3

15 10

2 1

5 0

Gax In1-x PyAs1-y /InP

0 4

k

ε2

20

329

n

ε1

OPTICAL PROPERTIES

(d) 2

3

4 E (eV)

5

6

0

2

3

4 E (eV)

5

6

Figure 10.27 Optical constants in the near-IR–UV region of GaxIn1xPyAs1y=InP at 300 K. The experimental data are taken from Adachi [3]

with (x, y) ¼ (0.734, 0.109) and (0.753, 0.093). These data agreed well with the theoretical prediction by Adachi [2,170]. From the far-field patterns in a GaxIn1xAsySb1y=AlxGa1xAsy Sb1y=GaSb double-heterostructure laser of lasing wavelength at 2.2 mm, Loural et al. [171] determined the active-layer n value to be 3.78. This value exactly agrees with the theoretical prediction based on the simplified interband-transition model [2,170]. Figure 10.28 shows the n(E) curves with x increments of 0.1 for (a) GaxIn1xAsySb1y/GaSb and (b) GaxIn1xAsySb1y/InAs calculated from the simplified interband-transition model [2,170].

Figure 10.28 n(E) dispersion in the transparent region of (a) GaxIn1xAsySb1y=GaSb and (b) GaxIn1x AsySb1y=InAs with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the simplified interband-transition model [2,170]

330

PROPERTIES OF SEMICONDUCTOR ALLOYS

The high-energy endpoint on each curve in Figure 10.28 corresponds to the n value at the band edge E0. A noticeable feature found in this figure is that these alloy systems show a refractive-index anomaly, i.e. the smaller E0-gap material has a smaller refractive index. Note that almost all III–V and II–VI semiconductor alloys, such as AlxGa1xAs and GaxIn1xPyAs1y, show no such anomalies in refractive-index (Figures 10.11 and 10.26).

10.4.3 (III, III, III)–V Alloy (a) AlGaInP The IR properties of (AlxGa1x)0.53In0.47P/GaAs have been studied by Hofmann et al. using far-IR SE [172]. They suggested that far-IR SE may be used to identify small degrees of longrange ordering in this quaternary. By fitting the SE n(E) data with the first-order Sellmeier equation, Adachi et al. [173] determined a set of the dispersion parameters A, B and C in the transparent region of the (AlxGa1x)0.53In0.47P quaternary that can be written as (C in mm) AðxÞ ¼ 5:38 þ 2:16x

ð10:11aÞ

BðxÞ ¼ 4:013:01x

ð10:11bÞ

CðxÞ2 ¼ 0:184 0:019x þ 0:024x2

ð10:11cÞ

As l ! ¥ in the fist-order Sellmeier equation, we obtain n(l ! ¥)2 ¼ «¥ ¼ A þ B. Figure 10.29 shows the n(E) dispersion with increments in x of 0.1 for (AlxGa1x)0.53 In0.47P/GaAs calculated from the simplified interband-transition model [2]. The solid circles represent the experimental data for x ¼ 0, 0.42 and 1.0 obtained by Tanaka et al. [174].

Figure 10.29 n(E) dispersion in the transparent region of (AlxGa1x)0.53In0.47P/GaAs with increments in x of 0.1 at 300 K, together with that for GaAs. The n(E) curves are calculated from the simplified interband-transition model [2]. The solid circles represent the experimental data for x ¼ 0, 0.42 and 1.0 reported by Tanaka et al. [174]

The optical constants in the interband transition region of (AlxGa1x)0.53In0.47P/GaAs have been measured by SE [3]. Figure 10.30 shows the complex optical constants, «(E) and n (E), taken from

20 15 10 5 0 -5 -10 25

(c)

3

1 4

(b)

3

15 k

ε2

4

2

x 0 0.25 0.50 0.75 1.00

20 10

(AlxGa1-x)0.53In0.47P/GaAs

(d)

2 1

5 0

331

5

(a) n

ε1

OPTICAL PROPERTIES

1

2

3

4

5

6

0

1

2

E (eV)

3

4

5

6

E (eV)

Figure 10.30 «(E)-related spectra in the IR–UV region of (AlxGa1x)0.53In0.47P/GaAs at 300 K. The experimental data are taken from Adachi [3]

Adachi [3]. The two major features seen in Figure 10.30 are due to the E1 and E2 CPs at 3.2–3.7 eV and 4.8 eV, respectively. The E1 structure moves toward higher energy with increasing x, while the E2 structure does not perceptibly do so. The E1 þ D1 structure is not clearly discernible in (AlxGa1x)0.53In0.47P/GaAs. These spectra were fitted by the MDF very well [175,176]. (b) AlGaInAs The n(E) dispersion in the transparent region and in the region a little above the E0 edge of (AlxGa1x)0.48In0.52As has been measured by several authors [3]. Figure 10.31 shows the experimental n(E) data for (AlxGa1x)0.48In0.52As/InP. These data are taken from Adachi [3]. Mondry et al. [82] modeled the experimental n(E) data with the first-order Sellmeier equation. The heavy solid lines in Figure 10.31 represent the endpoint ternary data that they obtained. The fundamental absorption edge in (AlxGa1x)0.48In0.52As/InP has been measured by Masu et al. [177]. The spectra showed a sharp decline in a(E), common to direct-band-gap 3.8 (AlxGa1-x)0.48In0.52As/InP

3.7 3.6

x=0 (GaInAs)

n

3.5 3.4

0.27

3.3 0.49 0.54

3.2 0.75 3.1 0.4

1.00 (AlInAs)

0.6

0.8 1.0 E (eV)

1.2

1.4

Figure 10.31 n(E) dispersion in (AlxGa1x)0.48In0.52As/InP at 300 K. The experimental data are taken from Adachi [3]. The heavy solid lines represent the endpoint ternary data by Mondry et al. [82]

332

PROPERTIES OF SEMICONDUCTOR ALLOYS

semiconductor materials. Using LPE Swarup et al. [178] also measured the absorption spectra of AlxGayIn1xyAs layers grown on the (111)As face of GaAs substrates. The optical constants in the interband transition region of (AlxGa1x)0.48In0.52As/InP have been determined using SE [3]. The refractive indices in the wavelength range 1.0–1.9 mm of (AlxGa1x)0.48In0.52As/InP have also been determined by SE [179]. The n(E) curves with increments in x of 0.1 for (AlxGa1x)0.48In0.52As/InP calculated from the simplified interbandtransition model [2] are shown in Figure 10.32.

Figure 10.32 n(E) dispersion in the transparent region of (AlxGa1x)0.48In0.52As/InP with increments in x of 0.1 at 300 K, together with that for InP. The n(E) curves are calculated from the simplified interband-transition model [2,3]

10.4.4 III–(V, V, V) Alloy A very limited number of reports are available for the optical properties of III–(V, V, V) quaternaries. The IR reflectivity spectra for InPxAsySb1xy layers grown on (111)InAs have been measured by Belov et al. [180]. The optical transmission measurements on LPE-grown InPxAsySb1xy/InAs have also been carried out by Esina et al. [181]. Adachi [3] calculated the n(E) dispersion in AlPxAsySb1xy, GaPxAsySb1xy and InPxAsySb1xy lattice-matched to GaAs, InP or InAs with increments in x of 0.1 using the simplified interband-transition model.

10.5 II–VI SEMICONDUCTOR ALLOY 10.5.1 (II, II)–O Ternary Alloy (a) BeZnO Transmittance measurements on BexZn1xO/sapphire samples have been carried out [182,183]. The measured spectra are used to determine the composition dependence of E0 (Figure 6.54(a)). (b) MgZnO The reststrahlen properties of MgxZn1xO have been investigated using far-IR reflectivity [184] and SE [185]. Variation in the optical phonon modes with x has been determined in the hexagonal and cubic regions [185].

OPTICAL PROPERTIES

333

The n(E) dispersion in w-MgxZn1xO has been determined for x in the hexagonal [186,187] and cubic regions [188,189]. The n values obtained by Teng et al. [187] have been reproduced in Figure 10.33. The thermo-optical coefficient dn/dT for c-MgxZn1xO (0.57 x 1.0) has also been determined by Zhou et al. [190].

Figure 10.33 Ordinary-ray (no) and extraordinary-ray refractive-index spectra (ne) for w-MgxZn1xO at 300 K, together with that for c-MgO. [Reprinted with permission from C. W. Teng et al., Appl. Phys. Lett. 76, 979 (2000). Copyright (2000), American Institute of Physics]

The absorption coefficient a(E) in the fundamental absorption edge of w-MgxZn1xO has been reported [187]. The pressure dependence of a(E) has also been reported [191]. The optical properties in the interband transition region of MgxZn1xO have been investigated using SE [186,192–194] and reflectivity [195]. The SE «(E) spectra for w-MgxZn1xO obtained by Kang et al. [192] have been reproduced in Figure 10.34. The n ¼ 1 excitonic peak can clearly be seen in the «(E) spectra. This is especially true for samples with low x. The higher-lying CPs can also be identified at 7 and 9 eV for x ¼ 0–0.53 [193]. (c) ZnCdO The optical absorption spectra a(E) in the fundamental absorption edge of CdxZn1xO have been measured by several authors [196–199]. The data were used to determine the composition dependence of E0 (Figure 6.54(c)).

10.5.2 (II, II)–S Ternary Alloy (a) MgZnS The optical absorption in w-MgxZn1xS has been measured for 0 x 0.25 [200]. The samples were grown on (0001)-sapphire substrates by PLD. The absorption edge showed blueshift with increasing x (Figure 6.55(a)).

334

PROPERTIES OF SEMICONDUCTOR ALLOYS 12

18 (a)

(b)

16

10 0.21

+9.5

12 0.14

+8.0

10 8

0.11

2

4

x=0

+4.0 0.11 +2.0 0.08

2 0

2.0 2.4 2.8 3.2 3.6 4.0 4.4 4.8 E (eV)

+7.0

0.14

6

+3.0

6 4

8

+5.0 0.08

w-MgxZn1-xO 0.21

ε2

ε1

14

+8.0

x=0 2.0 2.4 2.8 3.2 3.6 4.0 4.4 4.8 E (eV)

Figure 10.34 «(E) spectra for w-MgxZn1xO at 300 K. [Reprinted with permission from Solid State Commun., Spectroscopic ellipsometry study of Zn1–xMgxO thin films deposited on Al2O3(0001) by J. H. Kang, Y. R. Park and K. J. Kim, 115, 127–130. Copyright (2000), Elsevier]

(b) ZnCdS Transmittance and reflectance measurements in the reststrahlen region of w-ZnxCd1xS have been carried out by Lisitsa et al. [201]. The n(E) dispersion in c-ZnxCd1xS has also been studied by reflectivity measurements [202]. These results are reproduced in Figure 10.35. Optical absorption a(E) in the fundamental absorption edge of w-CdxZn1xS has been measured at 77 and 150 K [203]. The samples were grown by a sublimation method. The pressure

Figure 10.35 n(E) dispersion in the transparent region of c-ZnxCd1xS at 300 K. The dashed curves correspond to x ¼ 0.83, 0.91, 0.95 and 0.983 from right to left. [From P. Chen et al., Semicond. Sci. Technol. 13, 1439 (1998), Copyright (1998) Institute of Physics]

OPTICAL PROPERTIES

335

dependence of the fundamental absorption edge has also been measured on chemical-transportgrown w-CdxZn1xS layers up to their respective phase transition [204].

10.5.3 (II, II)–Se Ternary Alloy (a) BeZnSe The n(E) dispersion in c-BexZn1xSe layers grown on GaAs substrates by MBE has been measured using a prism coupler technique [205]. The data were fitted to the Sellmeier dispersion equation. These results are shown in Figure 10.36, together with the n(E) dispersion in ZnSe (x ¼ 0) [3]. 3.0 2.9

n

2.8

c-BexZn1-xSe

2.7

x=0 (ZnSe)

2.6 2.5 2.4 2.3 0.8

1.0

1.2

1.6

2.0 2.4 E (eV)

2.8

3.2

Figure 10.36 n(E) dispersion in the transparent region of c-BexZn1xSe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Peiris et al. [205]. The ZnSe data are taken from Adachi [3]

The optical properties of c-BexZn1xSe have been studied using SE in the spectral ranges 2.5–29 eV [206], 1.5–6.0 eV [207] and 1.255.0 eV [208]. The SE «2(E) spectra for c-BexZn1xSe with 0 x 1.0 and E ¼ 2.59 eV [206] are reproduced in Figure 10.37. The very weak structures due to the Zn 3d transitions were identified in the spectral region above 10 eV. (b) BeCdSe SE was used to obtain the «(E) spectra in the range of 0.756.5 eV for w-BexCd1xSe with x ¼ 0.075 [209,210]. The E0, E1 and E2 CPs were identified at 2, 4 and 6 eV, respectively. The alloys at x 0.1 were also grown, but they exhibited chemical instability. (c) MgZnSe The n(E) dispersion in c-MgxZn1xSe layers grown on GaAs(100) and silica glasses by MBE has been measured by Peiris et al. [211] and Derkowska et al. [212], respectively. Peiris et al. [211] reported the first-order Sellmeier constants as a function of x. The n(E) dispersion calculated using these constants, together with the experimental n(E) data for ZnSe (x ¼ 0) [3] are shown in Figure 10.38. The bold solid line is also obtained from the first-order Sellmeier parameters for ZnSe [213]. The absorption coefficients a(E) in the fundamental absorption edge of MBE-grown c-MgxZn1xSe/GaAs layers (0 x 0.36) have been measured at 2 K by W€orz et al. [214]. These results have been reproduced in Figure 10.39. The E0 and E0 þ D0 excitons can be

336

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.37 «2(E) spectra for c-BexZn1xSe at 300 K. [Reproduced with permission from K. Wilmers et al., J. Electron. Mater. 28, 670–677 (1999), Copyright (1999) Springer Science and Business Media]

clearly detected for x up to 0.28. The difference between the n ¼ 1 (1s) and 2 (2s) excitons yields the Rydberg energy

n

4 Ry* ¼ ðE1s E2s Þ 3 3.0 2.9 2.8 2.7 2.6 2.5 2.4 2.3 2.2 0.5

ð10:12Þ

c-MgxZn1-xSe x = 0 (ZnSe)

0.5

1.0

1.5

2.0 2.5 E (eV)

3.0

Figure 10.38 n(E) dispersion in the transparent region of c-MgxZn1xSe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Peiris et al. [211]. The bold solid line (ZnSe) is also calculated from the first-order Sellmeier parameters reported by Adachi [213]. The ZnSe data are taken from Adachi [3] (solid circles)

OPTICAL PROPERTIES

337

Figure 10.39 a(E) spectra in the fundamental absorption edge of MBE-grown c-MgxZn1xSe/GaAs layers (0 x 0.36) at 2 K. [Reprinted with permission from M. W€ orz et al., Phys. Status Solidi B 202, 805 (1997), Copyright (1997) Wiley–VCH]

which in this case, is equal to the exciton binding energy G. The composition dependence obtained by W€ orz et al. [214] can be written as G ¼ (20 0.2) þ (37.5 7)x meV. The optical properties in the interband transition region of c-MgxZn1xSe have been studied using SE [207,215]. The SE data analysis suggested that increasing x leads to a gradual increase in the E0/(E0 þ D0) and E1/(E1 þ D1) CP energies. (d) MgCdSe The optical properties of w-MgxCd1xSe (0 x 0.46) were investigated by optical absorption measurements at 300 K [216]. SE was also used to obtain the «(E) spectra for w-MgxCd1xSe in the range of 0.756.5 eV with x ¼ 0.15 and 0.29 [210] and in the range of 1.254.5 eV with x ¼ 00.40 [217]. (e) ZnCdSe The n(E) dispersion in c-ZnxCd1xSe has been measured by Peiris et al. [211,218]. These authors reported the first-order Sellmeier parameters as a function of x [211]. The n(E) dispersion calculated using these parameters are shown in Figure 10.40, together with the experimental ZnSe data [3]. The bold solid line also represents the first-order Sellmeier parameters for ZnSe obtained by Adachi [213]. A temperature shift of Dn/DT ¼ 1.0 104 K1 (T ¼ 50–300 K) has also been reported by analyzing laser emission wavelengths from a ZnxCd1xSe-based distributed feedback laser [219]. SE has been used to study the optical properties of c-ZnxCd1xSe by several groups [220– 223]. The samples used in these studies were epitaxial films grown by MBE on GaAs with x ¼ 0–1.0 [220], 0.75–1.0 [221] and 0.66–1.0 [222] and on InP with x ¼ 0.53 [223].

338

PROPERTIES OF SEMICONDUCTOR ALLOYS 3.0 2.9

n

2.8 2.7 2.6

c-CdSe

ZnSe

x=0

2.5 2.4 2.3 0.5

c-ZnxCd1-xSe

1.0

1.0

1.5

2.0 E (eV)

2.5

3.0

Figure 10.40 n(E) dispersion in the transparent region of c-ZnxCd1xSe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Peiris et al. [211]. The bold solid line (ZnSe) is also calculated from the first-order Sellmeier parameters reported by Adachi [213]. The c-CdSe (x ¼ 0) and ZnSe (x ¼ 1.0) data are taken from Adachi [3]

Suzuki and Adachi [224] used the MDF calculation to obtain a closed analytic formula for the optical constants of c-ZnxCd1xSe as a function of x. Figure 10.41 shows the MDFcalculated n(E) spectra in the region below and above the E0/(E0 þ D0) edge of c-ZnxCd1xSe with increments in x of 0.2 [224]. The solid and open circles represent the experimental data taken from Adachi [3] (ZnSe) and Holden et al. [223] (Zn0.53Cd0.47Se), respectively.

Figure 10.41 Theoretical n(E) spectra in the region below and above the E0/(E0 þ D0) edge of c-Znx Cd1xSe with increments in x of 0.2 at 300 K. The black and gray circles represent the experimental data for ZnSe and Zn0.53Cd0.47Se, respectively. [Reprinted with permission from K. Suzuki and S. Adachi, J. Appl. Phys. 83, 1018 (1998). Copyright (1998), American Institute of Physics]

(f) CdHgSe IR reflectivity spectra of c-CdxHg1xSe (x ¼ 0–0.32) have been reported by Kumazaki et al. [225]. They found that the measured reflectivity can be explained by the dynamic dielectric function constructed as the sum of the interband, intraband and phonon contributions.

OPTICAL PROPERTIES

339

The temperature and composition dependence of n in the transparent region of c-CdxHg1xSe has been determined by means of a fringe-spacing analysis [226]. The optical absorption properties near the fundamental absorption edge of c- and w-CdxHg1xSe have also been reported [226–229]. The fundamental reflectivity spectra for c-CdxHg1xSe have been measured [230]. The SE «(E) spectra for c-CdxHg1xSe (x ¼ 0–0.3) have also been measured in the 1.7–5.6 eV region at 300 K [231].

10.5.4 (II, II)–Te Ternary Alloy (a) BeZnTe The optical properties in the interband transition region of BexZn1xTe have been investigated using reflectivity [232]. The x dependence of E0 has been determined from this study. SE has also been used to measure «2(E) in BexZn1xTe [233–235]. (b) MgZnTe

n

The n(E) dispersion in c-MgxZn1xTe layers (0 x 0.67) grown on GaAs(100) by MBE has been determined from reflectivity measurements [236]. Figure 10.42 shows the n(E) dispersion calculated using first-order Sellmeier parameters [236], together with the experimental ZnTe data [3]. The bold solid line (ZnTe) has also been calculated using first-order Sellmeier parameters [213]. 3.3 3.2 3.1 3.0 2.9 2.8 2.7 2.6 2.5 2.4 2.3

0.5

c-MgxZn1-xTe x=0 (ZnTe)

0.7

0

0.5

1.0

1.5 2.0 E (eV)

2.5

3.0

Figure 10.42 n(E) dispersion in the transparent region of c-MgxZn1xTe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Liu et al. [236]. The bold solid line (ZnTe) is also calculated from the first-order Sellmeier parameters reported by Adachi [213]. The experimental data are taken from Adachi [3] (solid circles)

The optical absorption coefficients a(E) in the fundamental absorption edge of bulk c-MgxZn1xT crystals (0 x 0.48) grown by the Bridgman method have been measured at 4.2 K [237]. These results have been reproduced in Figure 10.43. The n ¼ 1 (1s) excitonic peak can be clearly seen at the E0 edge of each sample. SE measurements have been carried out on MBE-grown c-ZnxCd1xSe/GaAs(100) layers (0 x 0.52) [238]. The composition dependence of the excitonic E0, E0 þ D0 and E2 gaps has been determined in this study.

340

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 10.43 a(E) spectra in the fundamental absorption edge of c-MgxZn1xTe (0 x 0.48) at 4.2 K. [Reprinted with permission from S.-J. Chung et al., J. Phys. Chem. Solids 60, 799–805 (1999), Copyright (1999) Elsevier]

(c) MgCdTe The IR reflectivity spectra for c-MgxCd1xTe with x ¼ 00.6 have been measured in the range of 100–500 cm1 at 300 K [239]. The n(E) dispersion in c-MgxCd1xTe has also been measured at 4 K by Andre and Dang [240], at 77 and 300 K by Lugauer et al. [241] and at 300 K by Luttmann et al. [242]. Figure 10.44 shows the n(E) spectra calculated from first-order Sellmeier parameters by Luttmann et al. [242], together with the experimental CdTe n(E) data taken from Adachi [3]. 3.6 3.4

c-MgxCd1-xTe

n

3.2 3.0

x = 0 (CdTe)

0.5

2.8 1.0

2.6 2.4 2.2

0

0.5 1.0 1.5 2.0 2.5 3.0 3.5 E (eV)

Figure 10.44 n(E) dispersion in the transparent region of c-MgxZn1xTe with increments in x of 0.1 at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters reported by Luttmann et al. [242]. The experimental CdTe data are taken from Adachi [3]

SE measurements have been performed to determine the «(E) spectra for c-MgxCd1xTe [242–244]. The composition-dependent higher-order CPs, such as E1, E1 þ D1 and E2, have been determined from these «(E) spectra. (d) ZnCdTe The IR reflectivity in the reststrahlen region of ZnxCd1xTe has been measured by several authors [245–248]. The n(E) dispersion in ZnxCd1xTe has also been measured at room

OPTICAL PROPERTIES

341

3.3 3.2

0.8

ZnxCd1-xTe 0.5

3.1 n

0.3

3.0 2.9

x = 0 (CdTe)

1.0 (ZnTe)

2.8 2.7 0.5

1.0

1.5 E (eV)

2.0

2.5

Figure 10.45 n(E) dispersion in the transparent region of ZnxCd1xTe at 300 K. The n(E) curves are calculated from the first-order Sellmeier parameters [249]. The open circles represent the CdTe (x ¼ 0) and ZnTe (x ¼ 1.0) data taken from Adachi [3]

temperature in the 1.1–2.5 eV range by Adachi and Kimura [249]. The samples used by these authors were grown by the conventional Bridgman method. These results have been reproduced in Figure 10.45. The optical absorption spectra in the near-IR and mid-IR regions of ZnxCd1xTe have been measured at 300 K [250–252] and at 2 K [252]. The absorption coefficients a(E) are found to exhibit an exponential dependence on E according to the Urbach rule [251]. The room-temperature reflectivity spectra in the interband transition region of ZnxCd1xTe have been measured by several authors [253–256]. The R(E) spectra revealed the higherlying CPs, E0, E1, E1 þ D1, etc. The optical properties in the interband transition region of ZnxCd1xTe have also been investigated using SE [257–260]. The n(E) and k(E) spectra obtained by Adachi and Kimura have been reproduced in Figure 10.46 [257]. These spectra were parameterized to enable the calculation of the optical response in a ZnxCd1xTe alloy having an arbitrary composition x and photon energy E.

Figure 10.46 n(E) and k(E) spectra for ZnxCd1xTe with x ¼ 0, 0.3, 0.5, 0.8 and 1.0 at 300 K. [Reprinted with permission from Jpn. J. Appl. Phys., Optical constants of Zn1xCdxTe ternary alloys: Experiment and modeling by S. Adachi and T. Kimura, 32, 3496. Copyright (1993), Institute of Pure and Applied Physics]

342

PROPERTIES OF SEMICONDUCTOR ALLOYS

(e) ZnHgTe The IR optical properties of ZnxHg1xTe have been studied by a number of authors [261–264]. The absorption coefficients a(E) in the fundamental absorption edge of ZnxHg1xTe have also been measured by several authors [264–266]. SE has been carried out on ZnxHg1xTe in the range between 0.75 and 5.7 eV by Castaing et al. [267]. (f) CdHgTe The optical properties in the reststrahlen region of CdxHg1xTe have been investigated by a number of groups [263,268–271]. The a(E) spectra in the IR region have also been measured by a number of authors [272–278]. An empirical formula for the intrinsic optical absorption coefficient in the Kane region is given by Chu et al. [279]. The n(E) dispersion in CdxHg1xTe has been measured at different temperatures from 77 up to 350 K [273,275,280,281]. Figure 10.47 shows the results obtained by Kucera [280]. Liu et al. [281] also obtained n(l, T) from transmittance interference spacing nðl; TÞ2 ¼ A þ

B 2

1ðC=lÞ

þ Dl2

ð10:13Þ

Figure 10.47 n(E) dispersion in CdxHg1xTe with x ¼ 0.180–1.000 at 300 K. [Reprinted with permission from Z. Kucera, Phys. Status Solidi A 100, 659–665 (1987), Copyright (1987) Wiley–VCH]

where l is the wavelength and A, B, C and D are fitting parameters which vary with composition x and temperature T. This formula can be used for x ¼ 0.200–0.443 at T ¼ 4.2–300 K. The formula can also be used with x 0.540 at different temperatures and with x ¼ 0.54–1.0 at room temperature. The fundamental reflectivity spectra in the interband transition region of CdxHg1xTe have been measured at 315 K by Gał azka ˛ and Kisiel [282] and at 115–300 K by Rodzik and Kisiel [283]. The optical properties of CdxHg1xTe have also been studied using SE in the 1.8–5.5 eV spectral region by Vi~ na et al. [284] and in the 1.5–6.0 eV region by Arwin and Aspnes [285]. The dependence of «(E) on T has been discussed by Kim and Sivananthan [286] and Johs et al. [287].

OPTICAL PROPERTIES

343

10.5.5 Zn–(VI, VI) Ternary Alloy (a) ZnOS A series of w-ZnOxS1x films with 0 x 1.0 were deposited by rf reactive sputtering on different substrates [288] and the composition dependence of E0 was then determined from optical transmission measurements (Figure 6.59(a)). (b) ZnSSe The IR reflectivity and absorption in c-ZnSxSe1x have been measured by several authors [289,290]. The n(E) and k(E) curves for c-ZnSxSe1x have also been determined from optical transmittance measurements [291]. Ozaki and Adachi [292] carried out MDF analysis to obtain a closed analytic formula for the optical constants of c-ZnSxSe1x as a function of x. Figure 10.48 shows the MDF-calculated n(E) dispersion in the E0/(E0 þ D0) region of c-ZnSxSe1x with increments in x of 0.1 [292].

Figure 10.48 n(E) dispersion in the transparent region of c-ZnSxSe1x with increments in x of 0.1 at 300 K. The n(E) curves are obtained from the MDF calculation. [Reprinted with permission from S. Ozaki and S. Adachi, J. Appl. Phys. 75, 7470 (1994). Copyright (1994), American Institute of Physics]

The low-temperature absorption coefficients a(E) in the E0 region of MOCVD-grown c-ZnSxSe1x layers were measured by Gebhard and Sch€otz [293]. The hydrostatic-pressure dependent a(E) spectra were also reported by the same authors [294]. The room-temperature R(E) spectra in the interband transition region of c-ZnSxSe1x were measured by Ebina et al. [295]. Several peaks related to the higher-lying CPs were determined as a function of x. The R values (0.3) are, however, considerably smaller than those obtained by Ozaki and Adachi [292], suggesting that the sample surfaces used by Ebina et al. were of poorer quality. Jans et al. [221] carried out SE measurements on MBE-grown c-ZnSxSe1x/GaAs samples. They reported only the «(E) spectrum for ZnS0.15Se0.85. Ozaki and Adachi [292] presented the MDF-calculated «(E) spectra in the 16 eV region of c-ZnSxSe1x with increments in x of 0.2. (c) ZnSTe A strongly nonlinear pressure dependence of the band gaps and large downward shifts of the CB edges as a function of x in c-ZnSxTe1x has been found from optical transmittance

344

PROPERTIES OF SEMICONDUCTOR ALLOYS

data [296] (Figure 6.59(c)). SE has also been used to determine the «(E) spectra in the 1.5–6.0 eV region of c-ZnSxTe1x films deposited by hot-wall epitaxy [297]. (d) ZnSeTe The optical properties in the reststrahlen region of ZnSexTe1x have been measured by several authors [298,299]. A series of ZnSexTe1x films with 0 x 1.0 were grown on GaAs(100) substrates by MBE to determine the x dependence of n(E) [300]. Ozaki and Adachi [301] used the MDF method to obtain a closed analytic formula for the optical constants of ZnSexTe1x as a function of x. Figure 10.49 shows the MDF-calculated n(E) dispersion in the E0/(E0 þ D0) region of ZnSexTe1x with increments in x of 0.1 [301].

Figure 10.49 n(E) dispersion in the transparent region of ZnSexTe1x with increments in x of 0.1 at 300 K. The n(E) curves are obtained from the MDF calculation. [Reprinted with permission from Jpn. J. Appl. Phys., Optical constants of ZnSexTe1x ternary alloys by S. Ozaki and S. Adachi, 32, 2620–2625. Copyright (1993), Japanese Society of Applied Physics]

The hydrostatic-pressure dependent a(E) spectra were measured by Wu et al. [302]. The first- and second-order pressure coefficients of the fundamental absorption edge were determined as a function of x. The fundamental reflectivity spectra in the interband transition region of ZnSexTe1x were measured at 300 K by Ebina et al. [303]. The CP energies, such as E0, E0 þ D0, E1, E1 þ D1 and E2, were determined as a function of x. It should be noted however, that the R values (0.4) obtained were considerably smaller than those reported by Ozaki and Adachi [301], suggesting that Ebina et al. had used sample surfaces of inferior quality [303]. Ozaki and Adachi [301] also reported the MDF-calculated «(E) spectra in the 1–6 eV region of ZnSexTe1x with increments in x of 0.1.

10.5.6 Cd–(VI, VI) Ternary Alloy (a) CdSSe The optical properties in the reststrahlen region of w-CdSxSe1x have been studied by several authors [304–307]. The n(E) dispersion in the transparent region of w-CdSxSe1x has been measured with 0 x 1.0 in the temperature range between 100 and 600 K by

OPTICAL PROPERTIES

345

Figure 10.50 n(E) dispersion in the transparent region of w-CdSxSe1x with x ¼ 0, 0.36, 0.58, 0.79, 0.92 and 1.00 at 300 K. The solid and open symbols correspond to those for E?c (no) and E||c (ne), respectively. [Reprinted with permission from M. P. Lisitsa, L. F. Gudymenko, V. N. Malinko, and S. F. Terekhova, Phys. Status Solidi 31, 389 (1969), Copyright (1969) Wiley–VCH]

Lisitsa et al. [308]. These authors presented the results in a variety of graphical and tabular forms. The n(E) data at 300 K have been reproduced in Figure 10.50. The natural birefringence ne(E||c) > no(E?c) is evident for all samples investigated. Femtosecond time-resolved refractive-index changes in CdS0.75Se0.25 and CdS have also been measured using a pump–probe deflection technique [309]. The n(E) curves for polycrystalline CdSxSe1x films deposited on quartz substrates by pulsed-laser ablation technique have also been reported [310]. The a(E) spectra in the E0 region of w-CdSxSe1x have been measured for polarizations E?c and E||c [311]. The a(E) spectra for polycrystalline CdSxSe1x samples have also been reported [310]. The UV reflectivity of w-CdSxSe1x single crystals has been investigated at 90 K using linearly polarized light [312]. The x-dependent CPs, such as E1, E00, E2 and E10, were determined and correlated with the electronic dipole transitions in the BZ. (b) CdSTe Long-wavelength IR spectroscopy has been used to study the lattice vibrations in CdSxTe1x [313]. The sphalerite–wurtzite phase transition is found to occur in the x ¼ 0.20–0.25 range. The optical constants, n and a, of flash-evaporated CdSxTe1x films with 0 x 1.0 have been determined from reflectance and transmittance measurements [314]. As expected, the n value at l ¼ 2 mm decreased with increasing x. Thin films of polycrystalline CdSxTe1x (0 x 1.0) have also been prepared by vacuum evaporation. The complex refractive indices n ¼ n þ ik for these films have been determined in the wavelength range of 250–3200 nm from reflectance and transmittance measurements [315]. SE has been used to determine the optical constants in the IR–UV spectral region of polycrystalline CdSxTe1x films (0 x x1.0) grown on borosilicate glasses by PLD [316]. A modified MDF is used to analyze the measured SE spectra.

346

PROPERTIES OF SEMICONDUCTOR ALLOYS

(c) CdSeTe The IR reflectivity for Bridgman-grown CdSxSe1x (0 x x1.0) was investigated by several authors [317,318]. The composition dependence of the phonon frequencies did not show any discontinuity when the crystal structure changed from zinc-blende to wurtzite. More recently, Feng et al. [319] undertook IR reflectivity studies on CdSxSe1x (x 0.36). The samples used were grown by the Bridgman method and were single crystals with the zinc-blende structure. Optical constants, such as n and a, for CdSxSe1x in the limited composition ranges have also been reported [320–322].

10.5.7 (II, II)–(VI, VI) Quaternary Alloy (a) MgZnSSe The n(E) dispersion in MgxZn1xSySe1y/GaAs has been measured by several authors [323– 325]. These data showed that the smaller E0-gap material has a larger n value, as in many tetrahedral semiconductor alloys. The optical absorption in the fundamental absorption edge of MgxZn1xSySe1y/GaAs has also been measured by Lunz et al. [325]. SE has been used to determine the temperature dependence of E0 from 300 K to growth temperature in alloy compositions used in cladding layers and waveguides for blue–green light-emitting devices [326]. (b) MgZnSeTe The refractive index n at l ¼ 600 nm for MgxZn1xSeyTe1y/InP has been measured by Naniwae et al. [327]. The n value decreased almost linearly as the Mg content x increased in accordance with n ¼ 2.99–1.09x. The pressure-dependent absorption coefficients a(E) for MgxZn1xSeyTe1y have also been measured to investigate the band anticrossing effects [328], as popularly observed in dilute-nitride III–V alloys.

10.5.8 (II, II, II)–VI Quaternary Alloy (a) BeMgZnSe The n(E) dispersion in BexMgyZn1xySe/GaP has been measured at 300 K using SE [329]. The n value at l ¼ 370 nm decreased almost linearly as the alloy E0 value increased in accordance with n ¼ 4.61–0.49E0. SE has also been used to determine the composition dependence of CPs in BexMgyZn1xySe/GaAs [330]. (b) BeZnCdSe SE has been used to characterize bulk BexZnyCd1xySe grown by the Bridgman method [331]. The first-order Sellmeier equation is used to model the experimental n(E) data in the transparent region of the bulk alloys. (c) MgZnCdSe The n(E) dispersion in the transparent region of MgxZnyCd1xySe/InP has been measured by Morita et al. [332] and Guo et al. [333]. The experimental n(E) data obtained by Guo et al. [333] have been reproduced in Figure 10.51. These data were obtained using a prism coupler

OPTICAL PROPERTIES

347

Figure 10.51 n(E) dispersion in the transparent region of MgxZnyCd1xySe/InP at 300 K. [Reprinted with permission from S. P. Guo, O. Maksimov, M. C. Tamargo, F. C. Peiris, and J. K. Furdyna, Appl. Phys. Lett. 77, 4107 (2000). Copyright (2000), American Institute of Physics]

technique. Peiris et al. [334] also reported the refractive-index step Dn between MgxZnyCd1xySe and ZnxCd1xSe at l ¼ 632.8 nm.

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] S. Adachi, Optical Properties of Crystalline and Amorphous Semiconductors: Materials and Fundamental Principles, Kluwer Academic, Boston, 1999. [3] S. Adachi, Optical Constants of Crystalline and Amorphous Semiconductors: Numerical Data and Graphical Information, Kluwer Academic, Boston, 1999. [4] W. Kissinger, M. Weidner, H. J. Osten, and M. Eichler, Appl. Phys. Lett. 65, 3356 (1994). [5] H. Lee, S. R. Kurtz, J. A. Floro, J. Strane, C. H. Seager, S. R. Lee, E. D. Jones, J. F. Nelson, T. Mayer, and S. T. Picraux, Jpn. J. Appl. Phys. 34, L1340 (1995). [6] J. S. Schrader, J. L. Huguenin-Love, R. J. Soukup, N. J. Ianno, C. L. Exstrom, S. A. Darveau, R. N. Udey, and V. L. Dalal, Sol. Ener. Mater. Sol. Cells 90, 2338 (2006). [7] K. Kolodzey, P. A. O’Neil, S. Zhang, B. A. Orner, K. Roe, K. M. Unruh, C. P. Swann, M. M. Waite, and S. I. Shah, Appl. Phys. Lett. 67, 1865 (1995). [8] M. Krishnamurthy, K. -K. Yang, and W. H. Weber, Appl. Phys. Lett. 69, 2572 (1996). [9] R. Braunstein, Phys. Rev. 130, 879 (1963). [10] R. Braunstein, Phys. Rev. 130, 869 (1963). [11] R. Braunstein, A. R. Moore, and F. Herman, Phys. Rev. 109, 695 (195). [12] C. Pickering and R. T. Carline, J. Appl. Phys. 75, 4642 (1994). [13] J. C. Tsang, V. P. Kesan, J. L. Freeouf, F. K. LeGoues, and S. S. Iyer, Phys. Rev. B 46, 6907 (1992). [14] G. He and H. A. Atwater, Phys. Rev. Lett. 79, 1937 (1997). [15] H. P. L. de Guevara, A. G. Rodrıguez, H. Navarro-Contreras, and M. A. Vidal, Appl. Phys. Lett. 84, 4532 (2004).

348

PROPERTIES OF SEMICONDUCTOR ALLOYS

[16] H. P. L. de Guevara, A. G. Rodrıguez, H. Navarro-Contreras, and M. A. Vidal, Appl. Phys. Lett. 91, 161909 (2007). [17] V. R. D’Costa, C. S. Cook, A. G. Birdwell, C. L. Littler, M. Canonico, S. Zollner, J. Kouvetakis, and J. Menendez, Phys. Rev. B 73, 125207 (2006). [18] L. V. Kulik, C. Guedj, M. W. Dashiell, J. Kolodzey, and A. Hairie, Phys. Rev. B 59, 15753 (1999). [19] B. A. Orner, J. Olowolafe, K. Roe, J. Kolodzey, T. Laursen, J. W. Mayer, and J. Spear, Appl. Phys. Lett. 69, 2557 (1996). [20] H. Lee, J. A. Floro, J. Strane, S. R. Lee, E. D. Jones, T. Mayer, and S. T. Picraux, Mater. Res. Soc. Symp. Proc. 379, 211 (1995). [21] B.-K. Yang, M. Krishnamurthy, and W. H. Weber, J. Appl. Phys. 84, 2011 (1998). [22] S. Zollner, J. Hildreth, R. Liu, P. Zaumseil, M. Weidner, and B. Tillack, J. Appl. Phys. 88, 4102 (2000). [23] P. Aella, C. Cook, J. Tolle, S. Zollner, A. V. G. Chizmeshya, and J. Kouvetakis, Appl. Phys. Lett. 84, 888 (2004). [24] T. Suzuki, H. Yaguchi, H. Okumura, Y. Ishida, and S. Yoshida, Jpn. J. Appl. Phys. 39, L497 (2000). [25] U. K€ohler, D. J. As, B. Sch€ottker, T. Frey, K. Lischka, J. Scheiner, S. Shokhovets, and R. Goldhahn, J. Appl. Phys. 85, 404 (1999). [26] K. Torii, N. Usukura, A. Nakamura, T. Sota, S. F. Chichibu, T. Kitamura, and H. Okumura, Appl. Phys. Lett. 82, 52 (2003). [27] R. Goldhahn, J. Scheiner, S. Shokhovets, T. Frey, U. K€ ohler, D. J. As, and K. Lischka, Appl. Phys. Lett. 76, 291 (2000). [28] Z. G. Hu, M. Strassburg, N. Dietz, A. G. U. Perera, A. Asghar, and I. T. Ferguson, Phys. Rev. B 72, 245326 (2005). [29] K. Kazan, P. Masri, and M. Sumiya, J. Appl. Phys. 100, 013508 (2006). [30] U. Tisch, B. Meyler, O. Katz, E. Finkman, and J. Salzman, J. Appl. Phys. 89, 2676 (2001). € ur, H. O. Everitt, F. Yun, and H. Morko , Phys. Status Solidi A 188, 793 € Ozg€ [31] G. Webb-Wood, U. (2001). [32] R. Hui, S. Taherion, Y. Wan, J. Li, S. X. Jin, J. Y. Lin, and H. X. Jiang, Appl. Phys. Lett. 82, 1326 (2003). [33] N. Antoine-Vincent, F. Natali, M. Mihailovic, A. Vasson, J. Leymarie, P. Disseix, D. Byrne, F. Semond, and J. Massies, J. Appl. Phys. 93, 5222 (2003). [34] N. A. Sanford, L. H. Robins, A. V. Davydov, A. Shapiro, D. V. Tsvetkov, A. V. Dmitriev, S. Keller, U. K. Mishra, and S. P. DenBaars, J. Appl. Phys. 94, 2980 (2003). [35] N. Antoine-Vincent, F. Natali, M. Mihailovic, P. Disseix, A. Vasson, J. Leymarie, D. Byrne, F. Semond, and J. Massies, Phys. Status Solidi A 195, 543 (2003). [36] F. Omnes, N. Marenco, B. Beaumont, P. de Mierry, E. Monroy, F. Calle, and E. Mu~ noz, J. Appl. Phys. 86, 5286 (1999). [37] H. Angerer, D. Brunner, F. Freudenberg, O. Ambacher, M. Stutzmann, R. H€ opler, T. Metzger, E. Born, G. Dollinger, A. Bergmaier, S. Karsch, and H. -J. K€ orner, Appl. Phys. Lett. 71, 1504 (1997). [38] M. Stutzmann, O. Ambacher, A. Cros, M. S. Brandt, H. Angerer, R. Dimitrov, N. Reinacher, T. Metzger, R. H€opler, D. Brunner, F. Freudenberg, R. Handschuh, and C. Deger, Mater. Sci. Eng. B 50, 212 (1997). [39] T. Wethkamp, K. Wilmers, N. Esser, W. Richter, O. Ambacher, H. Angerer, G. Jungk, R. L. Johnson, and M. Cardona, Thin Solid Films 313–314, 745 (1998). [40] C. Buchheim, R. Goldhahn, M. Rakel, C. Cobet, N. Esser, U. Rossow, D. Fuhrmann, and A. Hangleiter, Phys. Status Solidi B 242, 2610 (2005). [41] T. Kawashima, H. Yoshikawa, S. Adachi, S. Fuke, and K. Ohtsuka, J. Appl. Phys. 82, 3528 (1997). [42] A. Kasic, M. Schubert, J. Off, and F. Scholz, Appl. Phys. Lett. 78, 1526 (2001). [43] G. M. Laws, E. C. Larkins, I. Harrison, C. Molloy, and D. Somerford, J. Appl. Phys. 89, 1108 (2001).

OPTICAL PROPERTIES

349

[44] Q. Guo, T. Tanaka, M. Nishio, and H. Ogawa, Jpn. J. Appl. Phys. 42, L141 (2003). [45] W. Terashima, S. -B. Che, Y. Ishitani, and A. Yoshikawa, Jpn. J. Appl. Phys. 45, L539 (2006). [46] R. Goldhahn, P. Schley, A. T. Winzer, G. Gobsch, V. Cimalla, O. Ambacher, M. Rakel, C. Cobet, N. Esser, H. Lu, and W. J. Schaff, Phys. Status Solidi A 203, 42 (2006). [47] K. Osamura, S. Naka, and Y. Murakami, J. Appl. Phys. 46, 3432 (1975). [48] N. A. Sanford, A. Munkholm, M. R. Kramers, A. Shapiro, I. Levin, A. V. Davydov, S. Sayan, L. S. Wielunski, and T. E. Madey, Phys. Status Solidi C 2, 2783 (2005). [49] T. Nagatomo, T. Kuboyama, H. Minamino, and O. Omoto, Jpn. J. Appl. Phys. 28, L1334 (1989). [50] C. A. Parker, J. C. Roerts, S. M. Bedair, M. J. Reed, S. X. Liu, N. A. El-Masry, and L. H. Robins, Appl. Phys. Lett. 75, 2566 (1999). [51] W. Walukiewicz, J. W. Ager III, K. M. Yu, Z. Liliental-Weber, J. Wu, S. X. Li, R. E. Jones, and J. D. Denlinger, J. Phys. D: Appl. Phys. 39, R83 (2006). [52] J. Wagner, A. Ramakrishnan, D. Behr, H. Obloh, M. Kunzer, and K. -H. Bachem, Appl. Phys. Lett. 73, 1715 (1998). [53] M. H. Lee, K. J. Kim, and E. Oh, Solid State Commun. 114, 325 (2000). [54] V. J. Keast, A. J. Scott, M. J. Kappers, C. T. Foxon, and C. J. Humphreys, Phys. Rev. B 66, 125319 (2002). [55] G. Lucovsky, R. D. Burnham, and A. S. Alimonda, Phys. Rev. B 14, 2503 (1976). [56] A. Onton, M. R. Lorenz, J. M. Woodall, and R. J. Chicotka, J. Cryst. Growth 27, 166 (1974). [57] P. Dias, V. A. Mishurnyi, E. L. Portnoi, B. S. Ryvkin, and V. B. Smirnitskii, Sov. Tech. Phys. Lett. 3, 290 (1977). [58] J. M. Rodrıguez and G. Armelles, J. Appl. Phys. 69, 965 (1991). [59] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, D. H. Woo, and S. H. Kim, J. Appl. Phys. 87, 1287 (2000). [60] G. Lucovsky, M. H. Brodsky, M. F. Chen, R. J. Chicotka, and A. T. Ward, Phys. Rev. B 4, 1945 (1971). [61] E. Jahne, W. Pilz, M. Giehler, and L. Hildisch, Phys. Status Solidi B 91, 155 (1979). [62] A. Hassine, J. Sapriel, P. L. Berre, P. Legay, F. Alexandre, and G. Post, J. Appl. Phys. 77, 6569 (1995). [63] A. R. Go~ni, K. Syassen, K. Str€ossner, and M. Cardona, Phys. Rev. B 39, 3178 (1989). [64] H. Lee, D. Biswas, M. V. Klein, H. Morkoç, D. E. Aspnes, B. D. Choe, J. Kim, and C. O. Grifﬁths, J. Appl. Phys. 75, 5040 (1994). [65] M. Schubert, V. Gottschalch, C. M. Herzinger, H. Yao, P. G. Snyder, and J. A. Woollam, J. Appl. Phys. 77, 3416 (1995). [66] R. Ferrini, G. Zuizzetti, M. Patrini, A. Parisini, L. Tarricone, and B. Valenti, Eur. Phys. J. B 27, 449 (2002). [67] D. H. Levi, J. F. Geisz, and B. Johs, Proc. SPIE 5530, 326 (2004). [68] S. Adachi, J. Appl. Phys. 58, R1 (1985). [69] D. E. Aspnes, S. M. Kelso, R. A. Logan, and R. Bhat, J. Appl. Phys. 60, 754 (1986). [70] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties. World Scientific, Singapore, 1994. [71] R. P. Seisyan, V. A. Kosobukin, S. A. Vaganov, M. A. Markosov, T. S. Shamirzaev, K. S. Zhuravlev, A. K. Bakarov, and A. I. Toropov, Phys. Status Solidi C 2, 900 (2005). [72] R. G. Kaufman, G. R. Hulse, D. J. Vezzetti, A. L. Moretti, K. A. Stair, G. P. Devane, and T. E. Bird, J. Appl. Phys. 75, 8053 (1994). [73] J. -H. Shin, and Y. -H. Lee, J. Appl. Phys. 76, 8048 (1994). [74] R. J. Deri and M. A. Emanuel, J. Appl. Phys. 77, 4667 (1995). [75] Y. Kokubo and I. Ohta, J. Appl. Phys. 81, 2042 (1997). [76] S. Gehrsitz, F. K. Reinhart, C. Gourdon, N. Herres, A. Vonlanthen, and H. Sigg, J. Appl. Phys. 87, 7825 (2000).

350

PROPERTIES OF SEMICONDUCTOR ALLOYS

[77] Z. G. Hu, M. B. M. Rinzan, S. G. Matsik, A. G. U. Perera, G. Von Winckel, A. Stintz, and S. Krishna, J. Appl. Phys. 97, 093529 (2005). [78] C. H. Kuo, S. Anand, H. Fathollahnejad, R. Ramamurti, R. Droopad, and G. N. Maracas, J. Vac. Sci. Technol. B 13, 681 (1995). [79] S. -J. Cho, and P. G. Snyder, J. Vac. Sci. Technol. B 17, 2045 (1999). Matyas, Sov. Phys. Semicond. 13, 1194 (1979). [80] E. [81] P. Roura, M. Lopez-de Miguel A. Cornet, and J. R. Morante, J. Appl. Phys. 81, 6916 (1997). [82] M. J. Mondry, D. I. Babic, J. E. Bowers, and L. A. Coldren, IEEE Photon. Technol. Lett. 4, 627 (1992). [83] H. Asai and H. Iwamura, Inst. Phys. Conf. Ser. 145, 985 (1996). [84] J. -H. Baek, B. Lee, S. W. Choi, J. H. Lee, and E. -H. Lee, Appl. Phys. Lett. 68, 2355 (1996). [85] H. W. Dinges, H. Burkhard, R. L€osch, H. Nickel, and W. Schlapp, Appl. Surf. Sci. 54, 477 (1992). [86] L. I. Kamlet, F. L. Terry, Jr., Thin Solid Films 313–314, 177 (1998). [87] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons, Ltd, New York, 1992. [88] G. Yu, N. L. Rowell, D. J. Lockwood, and P. J. Poole, Appl. Phys. Lett. 81, 2175 (2002); erratum, ibid. 82, 1136 (2003). [89] G. Yu, N. L. Rowell, D. J. Lockwood, and P. J. Poole, Appl. Phys. Lett. 86, 221904 (2005). [90] D. J. Lockwood, G. Yu, N. L. Rowell, and P. J. Poole, J. Appl. Phys. 101, 113524 (2007). [91] G. W. Charache, D. M. DePoy, J. E. Raynolds, P. F. Baldasaro, K. E. Miyano, T. Holden, F. H. Pollak, P. R. Sharps, M. L. Timmons, C. B. Geller, W. Mannstadt, R. Asahi, A. J. Freeman, and W. Wolf, J. Appl. Phys. 86, 452 (1999). [92] T. Takagi, Jpn. J. Appl. Phys. 17, 1813 (1978). [93] T. J. Kim, T. H. Ghong, Y. D. Kim, D. E. Aspnes, T. Mori, T. Yao, and B. H. Koo, Phys. Rev. B 68, 115323 (2003). [94] T. J. Kim, T. H. Ghong, and Y. D. Kim, J. Kor. Phys. Soc. 44, 726 (2004). [95] R. T. Carline, C. Pickering, N. S. Garawal, D. Lancefield, L. K. Howard, and M. T. Emeny, Proc. SPIE 1678, 285 (1992). [96] V. A. Yakovlen, Mater. Res. Soc. Symp. Proc. 340, 373 (1994). [97] L. C. Andreani, D. D. Nova, S. D. Lernia, M. Geddo, G. Guizzetti, M. Patrini, C. Bocchi, A. Bosacchi, C. Ferrari, and S. Franchi, J. Appl. Phys. 78, 6745 (1995). [98] M. Geddo, G. Guizzetti, M. Patrini, T. Ciabattoni, L. Seravalli, P. Frigeri, and S. Franchi, Appl. Phys. Lett. 87, 263120 (2005). [99] G. Lucovsky, K. Y. Cheng, and G. L. Pearson, Phys. Rev. B 12, 4135 (1975). [100] N. Kitamura and T. Wada, Mater. Lett. 19, 105 (1994). [101] R. Ferrini, M. Galli, G. Guizzetti, M. Patrini, A. Bosacchi, S. Franchi, and R. Magnanini, Phys. Rev. B 56, 7549 (1997). [102] R. Ferrini, M. Patrini, and S. Franchi, J. Appl. Phys. 84, 4517 (1998). [103] C. Ance and A. N. Van Mau, J. Phys. C: Solid State Phys. 9, 1565 (1976). [104] A. Bignazzi, E. Grilli, M. Guzzi, C. Bocchi, A. Bosacchi, S. Franchi, and R. Magnanini, Phys. Rev. B 57, 2295 (1998). [105] S. Dilernia, M. Geddo, G. Guizzetti, M. Patrini, A. Bosacchi, S. Franchi, and R. Magnanini, Mat. Res. Soc. Symp. Proc. 406, 389 (1996). [106] S. G. Choi, C. J. Palmstrem, Y. D. Kim, S. L. Cooper, and D. E. Aspnes, J. Appl. Phys. 98, 104108 (2005). [107] M. H. Brodsky, G. Lucovsky, M. F. Chen, and T. S. Plaskett, Phys. Rev. B 2, 3303 (1970). [108] Z. C. Feng, S. Perkowitz, R. Rousina, and J. B. Webb, Can. J. Phys. 69, 386 (1991). [109] R. Rousina, C. Halpin, and J. B. Webb, J. Appl. Phys. 68, 2181 (1990). [110] S. Imai and S. Adachi, Jpn. J. Appl. Phys. 32, 3860 (1993). [111] G. Leibiger, V. Gottschalch, A. Kasic, and M. Schubert, Appl. Phys. Lett. 79, 3407 (2001).

OPTICAL PROPERTIES

351

[112] J. B. Wang, Z. F. Li, W. Lu, D. J. Chen, B. Shen, and Y. D. Zheng, J. Vac. Sci. Technol. A 22, 1956 (2004). [113] G. Y. Rudko, I. A. Buyanova, W. M. Chen, H. P. Xin, and C. W. Tu, Appl. Phys. Lett. 81, 3984 (2002). [114] I. A. Buyanova, M. Izadifard, A. Kasic, H. Arwin, W. M. Chen, H. P. Xin, Y. G. Hong, and C. W. Tu, Phys. Rev. B 70, 085209 (2004). [115] B. Fluegel, Y. Zhang, J. F. Geisz, and A. Mascarenhas, Phys. Rev. B 72, 073203 (2005). [116] G. Leibiger, V. Gottschalch, M. Schubert, G. Benndorf, and R. Schwabe, Phys. Rev. B 65, 245207 (2002). [117] K. Uesugi and I. Suemune, Jpn. J. Appl. Phys. 36, L1572 (1997). [118] R. Chtourou, F. Bousbih, S. B. Bouzid, F. F. Charfi, J. C. Harmand, G. Ungaro, and L. Largeau, Appl. Phys. Lett. 80, 2075 (2002). [119] U. Tisch, E. Finkman, and J. Salzman, Appl. Phys. Lett. 81, 463 (2002). [120] W. K. Hung, M. Y. Chern, Y. F. Chen, Z. L. Yang, and Y. S. Huang, Phys. Rev. B 62, 13028 (2000). M. Schubert, G. Leibiger, V. Gottschalch, and G. Wagner, J. Appl. Phys. 89, 294 (2001). [121] J. Sik, and M. Schubert, J. Appl. Phys. 89, 4927 [122] G. Leibiger, V. Gottschalch, B. Rheinl€ander, J. Sik, (2001). [123] P. H. Jefferson, T. D. Veal, L. F. J. Piper, B. R. Bennett, C. F. McConville, B. N. Murdin, L. Buckie, G. W. Smith, and T. Ashley, Appl. Phys. Lett. 89, 111921 (2006). [124] W. G. Bi and C. W. Yu, J. Appl. Phys. 80, 1934 (1996). [125] W. K. Hung, K. S. Cho, M. Y. Chern, Y. F. Chen, D. K. Shih, H. H. Lin, C. C. Lu, and T. R. Yang, Appl. Phys. Lett. 80, 796 (2002). [126] D. -K. Shih, H. -H. Lin, L. -W. Sung, T. -Y. Chu, and T. -R. Yang, Jpn. J. Appl. Phys. 42, 375 (2003). [127] H. Shimomura, T. Anan, and S. Sugou, J. Cryst. Growth 162, 121 (1996). [128] F. Saadallah, N. Yacoubi, F. Genty, and C. Alibert, J. Appl. Phys. 94, 5041 (2003). [129] G. D. Clark, Jr., N. Holonyak, Jr., Phys. Rev. B 156, 913 (1967). [130] H. C. Casey, Jr., J. Appl. Phys. 45, 2766 (1974). [131] A. N. Pikhtin, A. D. Yas’kov, Sov. Phys. Semicond. 14, 389 (1980). [132] R. J. Nelson, N. Holonyak, Jr., and W. O. Groves, Phys. Rev. B 13, 5415 (1976). [133] A. G. Thompson, J. C. Woolley, and M. Rubenstein, Can. J. Phys. 44, 2927 (1966). [134] K. J. Kim, M. H. Lee, J. H. Bahng, K. Shim, and B. D. Choe, J. Appl. Phys. 84, 3696 (1998). [135] G. Lucovsky and M. F. Chen, Solid State Commun. 8, 1397 (1970). [136] M. Yano, Y. Suzuki, T. Ishii, Y. Matsushita, and M. Kimata, Jpn. J. Appl. Phys. 17, 2091 (1978). [137] K. G. Merkel, V. M. Bright, M. A. Marciniak, C. L. A. Cerny, and M. O. Manasreh, Appl. Phys. Lett. 65, 2442 (1994). [138] R. Lukic-Zrnic, B. P. Gorman, R. J. Cottier, T. D. Golding, C. L. Littler, and A. G. Norman, J. Appl. Phys. 92, 6939 (2002). [139] N. N. Sirota and E. E. Matyas, Phys. Status Solidi A 4, K143 (1971). [140] R. Ferrini, M. Geddo, G. Guizzetti, M. Patrini, S. Franchi, C. Bocchi, F. Germini, A. Baraldi, and R. Magnanini, J. Appl. Phys. 86, 4706 (1999). [141] D. Serries, M. Peter, N. Herres, K. Winkler, and J. Wagner, J. Appl. Phys. 87, 8522 (2000). [142] N. P. Kekelidze, G. P. Kekelidze, and Z. D. Makharadze, J. Phys. Chem. Solids 34, 2117 (1973). [143] D. J. Lockwood, N. L. Rowell, and G. Yu, J. Appl. Phys. 102, 033512 (2007). [144] I. V. Bodnar, A. I. Lukomskii, and G. F. Smirnova, Phys. Status Solidi A 37, K173 (1976). [145] S. G. Choi, C. J. Palmstrøm, Y. D. Kim, D. E. Aspnes, H. J. Kim, and Y. -C. Chang, Appl. Phys. Lett. 91, 041917 (2007). [146] E. H. Reihlen, M. J. Jou, Z. M. Fang, and G. B. Stringfellow, J. Appl. Phys. 68, 4604 (1990). [147] N. L. Rowell, D. J. Lockwood, G. Yu, Y. Z. Gao, X. Y. Gong, M. Aoyama, and T. Yamaguchi, J. Vac. Sci. Technol. A 22, 935 (2004). [148] M. B. Thomas and J. C. Woolley, Can. J. Phys. 49, 2052 (1971). [149] W. Dobbelaere, J. D. Boeck, and G. Borghs, Appl. Phys. Lett. 55, 1856 (1989).

352

PROPERTIES OF SEMICONDUCTOR ALLOYS

[150] V. K. Dixit, B. Bansal, V. Venkataraman, H. L. Bhat, K. S. Chandrasekharan, and B. M. Arora, J. Appl. Phys. 96, 4989 (2004). [151] M. A. Marciniak, R. L. Hengehold, Y. K. Yeo, and G. W. Turner, J. Appl. Phys. 84, 480 (1998). [152] G. B. Stringfellow and P. E. Greene, J. Electrochem. Soc. 118, 805 (1971). [153] H. Y. Deng and N. Dai, Phys. Rev. B 73, 113102 (2006). [154] Y. Z. Gao, X. Y. Gong, and T. Yamaguchi, Jpn. J. Appl. Phys. 45, 5732 (2006). [155] T. Imanishi, A. Wakahara, S. M. Kim, H. Yonezu, and Y. Furukawa, Phys. Status Solidi A 202, 854 (2005). [156] G. Leibiger, V. Gottschalch, and M. Schubert, J. Appl. Phys. 90, 5951 (2001). [157] C. Skierbiszewski, Semicond. Sci. Technol. 17, 803 (2002). [158] T. Kitatani, M. Kondow, K. Shinoda, Y. Yazawa, and M. Okai, Jpn. J. Appl. Phys. 37, 753 (1998). [159] P. N. Sen and G. Lucovsky, Phys. Rev. B 12, 2998 (1975). [160] V. V. Kuznetsov, V. N. Razbegaev, S. El-Giziri, Sov. Phys. Semicond. 23, 552 (1989). [161] A. Mezerreg, C. Llinares, J. L. Lazzari, and A. Montaner, Thin Solid Films 221, 196 (1992). [162] C. Alibert, M. Skouri, A. Joullie, M. Benouna, and S. Sadiq, J. Appl. Phys. 69, 3208 (1991). [163] O. Blum, I. J. Fritz, L. R. Dawson, and T. J. Drummond, Electron. Lett. 31, 1247 (1995). [164] P. Swarup, R. K. Jain, S. N. Verma, S Charan,h. and D. M. Tandle, Phys. Status Solidi A 65, K183 (1981). [165] F. Fiedler and A. Schlachetzki, Solid-State Electron. 30, 73 (1987). [166] S. M. Kelso, D. E. Aspnes, M. A. Pollack, and R. E. Nahory, Phys. Rev. B 26, 6669 (1982). [167] S. G. Wallace, B. J. Robinson, P. Mascher, H. K. Haugen, D. A. Thompson, D. Dalacu, and L. Martinu, Appl. Phys. Lett. 76, 2791 (2000). [168] C. Pickering, J. Electron. Mater. 15, 51 (1986). [169] W. G. Bi, A. Z. Li, and S. S. Tan, Mat. Res. Soc. Symp. Proc. 216, 213 (1991). [170] S. Adachi, J. Appl. Phys. 61, 4869 (1987). [171] M. S. S. Loural, M. B. Z. Morosini, J. L. Herrera-Perez, A. A. G. Von Zuben, A. C. F. da Silveir, and N. B. Patel, Electron. Lett. 29, 1240 (1993). [172] T. Hofmann, G. Leibiger, V. Gottschalch, I. Pietzonka, and M. Schubert, Phys. Rev. B 64, 155206 (2001). [173] S. Adachi, H. Kato, A. Moki, and K. Ohtsuka, J. Appl. Phys. 75, 478 (1994). [174] H. Tanaka, Y. Kawamura, and H. Asahi, J. Appl. Phys. 59, 985 (1986). [175] S. Ozaki, S. Adachi, M. Sato, and K. Ohtsuka, J. Appl. Phys. 79, 439 (1996). [176] M. Schubert, J. A. Woollam, G. Leibiger, B. Rheinl€ander, I. Pietzonka, T. Sab, and V. Gottschalch, J. Appl. Phys. 86, 2025 (1999). [177] K. Masu, T. Mishima, S. Hiroi, M. Konagai, and K. Takahashi, J. Appl. Phys. 53, 7558 (1982). [178] P. Swarup, R. K. Jain, S. N. Verma, S. Charan, and D. M. Tandle, Phys. Status Solidi A 72, K189 (1982). [179] H. W. Dinges, H. Burkhard, R. L€osch, H. Nickel, and W. Schlapp, Mater. Sci. Eng. B 21, 174 (1993). [180] A. G. Belov, G. M. Zinger, M. A. II’in, Yu. N. Korchagin, E. P. Rashevskaya, and A. I. Ryskin, Sov. Phys. Solid State 22, 839 (1980). [181] N. P. Esina, N. V. Zotova, B. A. Matveev, L. D. Neulmina, N. M. Stus’, and G. N. Talalakin, Sov. Phys. Semicond. 15, 1372 (1981). [182] Y. R. Ryu, T. S. Lee, J. A. Lubguban, A. B. Corman, H. W. White, J. H. Leem, M. S. Han, Y. S. Park, C. J. Youn, and W. J. Kim, Appl. Phys. Lett. 88, 052103 (2006). [183] M. S. Han, J. H. Kim, T. S. Jeong, J. M. Park, C. J. Youn, J. H. Leem, and Y. R. Ryu, J. Cryst. Growth 303, 506 (2007). [184] J. Chen and W. Z. Shen, Appl. Phys. Lett. 83, 2154 (2003). [185] C. Bundesmann, A. Rahm, M. Lorenz, M. Grundmann, and M. Schubert, J. Appl. Phys. 99, 113504 (2006). [186] R. Schmidt, B. Rheinl€ander, M. Shubert, D. Spemann, T. Butz, J. Lenzner, E. M. Kaidashev, M. Lorenz, A. Rahm, H. C. Semmelhack, and M. Grundmann, Appl. Phys. Lett. 82, 2260 (2003).

OPTICAL PROPERTIES

353

€ ur, M. J. Bergmann, H. O. Everitt, A. K. Sharma, C. Jin, and € Ozg€ [187] C. W. Teng, J. F. Muth, U. J. Narayan, Appl. Phys. Lett. 76, 979 (2000). [188] R. Schmidt-Grund, A. Carstens, B. Rheinl€ander, D. Spemann, H. Hochmut, G. Zimmermann, M. Lorenz, M. Grundmann, C. M. Herzinger, and M. Schubert, J. Appl. Phys. 99, 123701 (2006). [189] P. Yu, H. Wu, N. Chen, T. Xu, Y. Lao, and J. Liang, Opt. Mater. 28, 271 (2006). [190] H. P. Zhou, W. Z. Shen, N. B. Chen, and H. Z. Wu, Appl. Phys. Lett. 85, 3723 (2004). [191] J. A. Sans and A. Segura, High Pressure Res. 24, 119 (2004). [192] J. H. Kang, Y. R. Park, and K. J. Kim, Solid State Commun. 115, 127 (2000). [193] R. Schmidt-Grund, M. Schubert, B. Rheinl€ander, D. Fritsch, H. Schmidt, E. M. Kaidashev, M. Lorenz, C. M. Herzinger, and M. Grundmann, Thin Solid Films 455–456, 500 (2004). [194] T. D. Kang, H. Lee, W. -I. Park, and G. -C. Yi, Thin Solid Films 455–456, 609 (2004). [195] H. Tampo, H. Shibata, K. Maejima, A. Yamada, K. Matsubara, P. Fons, S. Niki, T. Tainaka, C. Chiba, and H. Kanie, Appl. Phys. Lett. 91, 261907 (2007). [196] T. Makino, Y. Segawa, M. Kawasaki, A. Ohtomo, R. Shiroki, K. Tamura, T. Yasuda, and H. Koinuma, Appl. Phys. Lett. 78, 1237 (2001). [197] S. Y. Lee, Y. Li, J. -S. Lee, J. K. Lee, M. Nastasi, S. A. Crooker, Q. X. Jia, H. -S. Kang, and J. -S. Kang, Appl. Phys. Lett. 85, 218 (2004). [198] J. Ishihara, A. Nakamura, S. Shigemori, T. Aoki, and J. Temmyo, Appl. Surf. Sci. 244, 381 (2005). [199] X. J. Wang, I. A. Buyanova, W. M. Chen, M. Izadifard, S. Rawal, D. P. Norton S. J. Pearton, A. Osinsky, J. W. Dong, and A. Dabiran, Appl. Phys. Lett. 89, 151909 (2006). [200] H. C. Ong and J. Y. Dai, Appl. Phys. Lett. 81, 1444 (2002). [201] M. P. Lisitsa, M. Y. Valakh, and N. K. Konovets, Phys. Status Solidi 34, 269 (1969). [202] P. Chen, J. E. Nicholls, M. O’Neill, J. H. C. Hogg, B. Lunn, D. E. Ashenford, M. Fay, and A. G. Cullis, Semicond. Sci. Technol. 13, 1439 (1998). [203] M. R. Muhamad, Jpn. J. Appl. Phys. 32, 3385 (1993). [204] A. Beliveau and C. Carlone, Phys. Rev. B 41, 9860 (1990). [205] F. C. Peiris, U. Bindley, J. K. Furdyna, H. Kim, A. K. Ramdas, and M. Grimsditch, Appl. Phys. Lett. 79, 473 (2001). [206] K. Wilmers, T. Wethkamp, N. Esser, C. Cobet, W. Richter, V. Wagner, H. Lugauer, F. Fischer, T. Gerhard, M. Keim, and M. Cardona, J. Electron. Mater. 28, 670 (1999). [207] H. Lee, I. -Y. Kim, J. Powell, D. E. Aspnes, S. Lee, F. Peiris, and J. K. Furdyna, J. Appl. Phys. 88, 878 (2000). [208] A. Bukaluk, A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Łegowski, ˛ H. Me˛ czy nska, and J. Szatkowski, Appl. Surf. Sci. 175–176, 531 (2001). [209] A. A. Wronkowska, A. Wronkowski, F. Firszt, S. Łegowski, ˛ H. Me˛ czy nska, A. Marasek, and W. Paszkowicz, Phys. Status Solidi C 1, 641 (2004). [210] F. Firszt, A. A. Wronkowska, A. Wronkowski, S. Ł e˛ gowski, A. Marasek, H. M e˛ czy nska, M. Pawlak, W. Paszkowicz, K. Strzałkowski, and A. J. Zakrzewski, Cryst. Res. Technol. 40, 386 (2005). [211] F. C. Peiris, S. Lee, U. Bindley, and J. K. Furdyna, J. Appl. Phys. 86, 918 (1999). [212] B. Derkowska, B. Sahraoui, X. N. Phu, G. Glowacki, and W. Bala, Opt. Mater. 15, 199 (2000). [213] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [214] M. W€orz, E. Griebl, T. Reisinger, R. Flierl, B. Haserer, T. Semmler, T. Frey, and W. Gebhardt, Phys. Status Solidi B 202, 805 (1997). [215] K. J. Kim, M. H. Lee, J. H. Bahng, C. Y. Kwak, and E. Oh, Solid State Commun. 105, 17 (1998). [216] D. -H. Shin, C. -D. Kim, H. -H. Jang, S. -H. Choe, D. -T. Kim, C. -S. Yoon, and W. -T. Kim, J. Cryst. Growth 177, 167 (1997). [217] A. A. Wronkowska, A. Wronkowski, H. Arwin, F. Firszt, S. Łegowski, ˛ H. M e˛ czy nska, and J. Szatkowski, Vacuum 63, 233 (2001). [218] F. C. Peiris, S. Lee, U. Bindley, and J. K. Furdyna, J. Appl. Phys. 84, 5194 (1998).

354

PROPERTIES OF SEMICONDUCTOR ALLOYS

[219] M. Illing, G. Bacher, A. Forchel, D. Hommel, B. Jobst, and G. Landwehr, Appl. Phys. Lett. 67, 1 (1995). [220] Y. D. Kim, M. V. Klein, S. F. Ren, Y. C. Chang, H. Luo, N. Samarthj, and J. K. Furdyna, Phys. Rev. B 49, 7262 (1994). [221] J. C. Jans, J. Petruzzello, J. M. Gaines, and D. J. Olego, Proc. SPIE 1985, 260 (1993). [222] J. Lee, F. Flack, N. Samarth, and R. W. Collins, Appl. Opt. 36, 5372 (1997). [223] T. Holden, P. Ram, F. H. Pollak, and J. L. Freeouf, Phys. Rev. B 56, 4037 (1997). [224] K. Suzuki and S. Adachi, J. Appl. Phys. 83, 1018 (1998). [225] K. Kumazaki, N. Nishiguchi, and M. Cardona, Solid State Commun. 58, 425 (1986). [226] C. J. Summers and J. G. Broerman, Phys. Rev. B 21, 559 (1980). [227] P. S. Kireev and V. V. Volkov, Sov. Phys. Semicond. 7, 949 (1974). [228] N. Himei and J. Muto, J. Mater. Sci.: Mater. Electron. 11, 145 (2000). [229] V. B. Pujari, S. H. Mane, V. S. Karande, J. S. Dargad, and L. P. Deshmukh, Mater. Chem. Phys. 83, 10 (2004). [230] I. N. Borisov, P. S. Kireev, V. V. Mikhailin, and V. M. Bezborodova, Sov. Phys. Semicond. 5, 734 (1971). [231] K. Kumazaki, L. Vi~na, C. Umbach, and M. Cardona, Phys. Status Solidi B 156, 371 (1989). [232] O. Maksimov and M. C. Tamargo, Appl. Phys. Lett. 79, 782 (2001). [233] M. R. Buckley, F. C. Peiris, O. Maksimov, M. Mu~ noz, and M. C. Tamargo, Appl. Phys. Lett. 81, 5156 (2002). [234] M. Mu~noz, O. Maksimov, M. C. Tamargo, M. R. Buckley, and F. C. Peiris, Phys. Status Solidi C 1, 706 (2004). [235] J. S. de Almeida, and R. Ahuja, Appl. Phys. Lett. 89, 061913 (2006). [236] X. Liu, U. Bindley, Y. Sasaki, and J. K. Furdyna, J. Appl. Phys. 91, 2859 (2002). [237] S. -J. Chung, Y. Kwon, C. -S. Yoon, B. -H. Kim, D. Cha, C. -D. Kim, W. -T. Kim, and C. U. Hong, J. Phys. Chem. Solids 60, 799 (1999). [238] A. J. Franz, F. C. Peiris, X. Liu, U. Bindley, and J. K. Furdyna, Phys. Status Solidi B 241, 507 (2004). [239] S. Nakamura, T. Fukumoto, A. Mitsuishi, and K. Itoh, J. Phys. Soc. Jpn 35, 1437 (1973). [240] R. Andre and L. S. Dang, J. Appl. Phys. 82, 5086 (1997). [241] H. -J. Lugauer, F. Fischer, T. Litz, A. Waag, D. Hommel, and G. Landwehr, Semicond. Sci. Technol. 9, 1567 (1994). [242] M. Luttmann, F. Bertin, and A. Chabli, J. Appl. Phys. 78, 3387 (1995). [243] S. G. Choi, Y. D. Kim, S. D. Yoo, D. E. Aspnes, I. Miotkowski, and A. K. Ramdas, Appl. Phys. Lett. 71, 249 (1997). [244] Y. S. Ihn, T. J. Kim, T. H. Ghong, Y. D. Kim, D. E. Aspnes, and J. Kossut, Thin Solid Films 455–456, 222 (2004). [245] H. Harada and S. Narita, J. Phys. Soc. Jpn 30, 1628 (1971). [246] L. K. Vodop’yanov, E. A. Vinogradov, A. M. Blinov, and V. A. Rukavishnikov, Sov. Phys. Solid State 14, 219 (1972). [247] S. Perkowitz, L. S. Kim, and Z. C. Feng, Phys. Rev. B 42, 1455 (1990). [248] D. N. Talwar, Z. C. Feng, and P. Becla, Phys. Rev. B 48, 17064 (1993). [249] S. Adachi and T. Kimura, Jpn. J. Appl. Phys. 32, 3866 (1993). [250] A. Ebina, K. Saito, and T. Takahashi, J. Appl. Phys. 44, 3659 (1973). [251] A. J. Syllaios, P. -K. Liao, B. J. Greene, H. F. Schaake, H. -Y. Liu, and G. Westphal, J. Electron. Mater. 26, 567 (1997). [252] D. Ohlmann, M. Mazilu, R. Levy, and B. H€onerlage, J. Appl. Phys. 82, 1355 (1997). [253] A. Kisiel, Acta Phys. Polon. A 38, 691 (1970). [254] K. Saito, A. Ebina, and T. Takahashi, Solid State Commun. 11, 841 (1972). [255] S. G. Kroitoru, O. G. Maksimova, and V. V. Sobolev, Sov. Phys. Semicond. 9, 1191 (1976). [256] V. V. Sovolev, O. G. Maksimova, and S. G. Kroitoru, Phys. Status Solidi B 103, 499 (1981).

OPTICAL PROPERTIES [257] [258] [259] [260] [261] [262] [263] [264] [265] [266] [267] [268] [269] [270] [271] [272] [273] [274] [275] [276] [277] [278] [279] [280] [281] [282] [283] [284] [285] [286] [287] [288] [289] [290] [291] [292] [293] [294] [295] [296] [297] [298]

355

S. Adachi and T. Kimura, Jpn. J. Appl. Phys. 32, 3496 (1993). O. Castaing, R. Granger, J. T. Benhlal, and R. Triboulet, J. Phys.: Condens. Matter 8, 5757 (1996). E. M. Larramendi, E. Puron, and O. de Melo, Semicond. Sci. Technol. 17, 8 (2002). P. D. Paulson, B. E. McCandless, and R. W. Birkmire, J. Appl. Phys. 95, 3010 (2004). G. L. Bastard, R. Granger, S. Rolland, Y. Marqueton, and R. Triboulet, J. Phys. (France) 50, 3223 (1989). M. P. Volz, F. R. Szofran, S. L. Lehoczky, and C. -H. Su, Solid State Commun. 75, 943 (1990). D. Bagot, R. Granger, and S. Rolland, Phys. Status Solidi B 183, 395 (1994). C. -H. Wu, D. -Y. Chu, C. -Y. Sun, and T. -R. Yang, Jpn. J. Appl. Phys. 34, 4687 (1995). B. Toulouse, R. Granger, S. Rolland, and R. Triboulet, J. Phys. (France) 48, 247 (1987). F. El-Akkad, and A. R. Farhan, J. Phys. D: Appl. Phys. 28, 1958 (1995). O. Castaing, J. T. Benhlal, R. Granger, and R. Triboulet, J. Phys. I (France) 6, 907 (1996). J. Baars and F. Sorger, Solid State Commun. 10, 875 (1972). D. N. Talwar and M. Vandevyver, J. Appl. Phys. 56, 1601 (1984). S. P. Kozyrev, V. N. Pyrkov, L. K. Vodop’yanov, Sov. Phys. Solid State 34, 1984 (1992). S. P. Kozyrev, L. K. Vodopyanov, and R. Triboulet, Phys. Rev. B 58, 1374 (1998). M. W. Scott, J. Appl. Phys. 40, 4077 (1969). E. Finkman and Y. Nemirovsky, J. Appl. Phys. 50, 4356 (1979). L. D. Saginov, V. P. Ponomarenko, V. A. Fedirko, and V. I. Stafeev, Sov. Phys. Semicond. 16, 298 (1982). E. Finkman and S. E. Schacham, J. Appl. Phys. 56, 2896 (1984). J. Chu, Z. Mi, and D. Tang, J. Appl. Phys. 71, 3955 (1992). B. Li, J. H. Chu, Y. Chang, Y. S. Gui, and D. Y. Tang, Infrared Phys. Technol. 37, 525 (1996). V. Nathan, J. Appl. Phys. 83, 2812 (1998). J. Chu, B. Li, and D. Tang, J. Appl. Phys. 75, 1234 (1994). Z. Kucera, Phys. Status Solidi A 100, 659 (1987). K. Liu, J. H. Chu, and D. Y. Tang, J. Appl. Phys. 75, 4176 (1994). R. R. Gał azka ˛ and A. Kisiel, Phys. Status Solidi 34, 63 (1969). A. Rodzik and A. Kisiel, J. Phys. C: Solid State Phys. 16, 203 (1983). L. Vi~na, C. Umbach, M. Cardona, and L. Vodopyanov, Phys. Rev. B 29, 6752 (1984). H. Arwin and D. E. Aspnes, J. Vac. Sci. Technol. A 2, 1316 (1984). C. C. Kim and S. Sivananthan, J. Electron. Mater. 26, 561 (1997). B. Johs, C. M. Herzinger, J. H. Dinan, A. Cornfeld, and J. D. Benson, Thin Solid Films 313–314, 137 (1998). B. K. Meyer, A. Polity, B. Farangis, Y. He, D. Hasselkamp, T. Kr€amer, and C. Wang, Appl. Phys. Lett. 85, 4929 (2004). O. Brafman, I. F. Chang, G. Lengyel, S. S. Mitra, E. Carnall, Jr., Phys. Rev. Lett. 19, 1120 (1967). D. Schmeltzer, R. Beserman, and D. Slamovits, Phys. Rev. B 22, 4038 (1980). M. Ambrico, D. Smaldone, C. Spezzacatena, V. Stagno, G. Perna, and V. Capozzi, Semicond. Sci. Technol. 13, 1446 (1998). S. Ozaki and S. Adachi, J. Appl. Phys. 75, 7470 (1994). W. Gebhard, G. Sch€otz, in Properties of Wide Bandgap IIVI Semiconductors, EMIS Datareviews Series No. 17 (edited by R. Bhargava), INSPEC (IEE), London, 1997, p. 113. E. Griebl, G. F. Sch€otz, C. Birzer, W. Kerner, T. Reisinger, B. Hahn, and W. Gebhardt, Acta Phys. Polon. A 88, 995 (1995). A. Ebina, E. Fukunaga, and T. Takahashi, Phys. Rev. B 10, 2495 (1974). W. Walukiewicz, W. Shan, K. M. Yu, J. W. Ager III, E. E. Haller, I. Miotkowski, M. J. Seong, H. Alawadhi, and A. K. Ramdas, Phys. Rev. Lett. 85, 1552 (2000). C. Y. Bang, M. S. Lee, T. J. Kim, Y. D. Kim, D. E. Aspnes, Y. M. Yu, B. O, and Y. D. Choi, J. Kor. Phys. Soc. 39, 462 (2001). V. M. Burlakov, A. P. Litvinchuk, and V. N. Pyrkov, Sov. Phys. Solid State 27, 131 (1985).

356 [299] [300] [301] [302] [303] [304] [305] [306] [307] [308] [309] [310] [311] [312] [313] [314] [315] [316] [317] [318] [319] [320] [321] [322] [323] [324] [325] [326] [327] [328] [329] [330] [331] [332] [333] [334]

PROPERTIES OF SEMICONDUCTOR ALLOYS T. R. Yang and C. C. Lu, Physica B 284–288, 1187 (2000). F. C. Peiris, U. Bindley, and J. K. Furdyna, J. Electron. Mater. 30, 677 (2001). S. Ozaki and S. Adachi, Jpn. J. Appl. Phys. 32, 2620 (1993). J. Wu, W. Walukiewicz, K. M. Yu, W. Shan, J. W. Ager III, E. E. Haller, I. Miotkowski, A. K. Ramdas, and C. -H. Su, Phys. Rev. B 68, 033206 (2003). A. Ebina, M. Yamamoto, and T. Takahashi, Phys. Rev. B 6, 3786 (1972). J. F. Parrish, C. H. Perry, O. Brafman, I. F. Chang and S. S. Mitra, in II–VI Semiconducting Compounds (edited by D. G. Thomas), Benjamin, New York, 1967, p. 1164. H. W. Verleur and A. S. Barker, Jr., Phys. Rev. 155, 750 (1967). R. Beserman and M. Balkanski, Phys. Rev. B 1, 608 (1970). R. Beserman, Solid State Commun. 23, 323 (1977). M. P. Lisitsa, L. F. Gudymenko, V. N. Malinko, and S. F. Terekhova, Phys. Status Solidi 31, 389 (1969). E. C. Fox, E. J. Canto-Said, and H. M. van Driel, Appl. Phys. Lett. 59, 1878 (1991). G. Perna, S. Pagliara, V. Capozzi, M. Ambrico, and T. Ligonzo, Thin Solid Films 349, 220 (1999). M. S. Brodin, M. V. Kurik, and S. P. Yurtsenyuk, Sov. Phys. Solid State 7, 2516 (1966). R. L. Hengehold and C. R. Fraime, Phys. Rev. 174, 808 (1968). Y. A. Mityagin, V. G. Plotnichenko, L. K. Vodop’yanov, and L. D. Budennaya, Sov. Phys. Solid State 19, 1811 (1977). K. Ohata, J. Saraie, and T. Tanaka, Jpn. J. Appl. Phys. 12, 1641 (1973). D. A. Wood, D. W. Lane, K. D. Rogers, and J. A. Coath, J. Electron. Mater. 28, 1403 (1999). K. Wei, F. H. Pollak, J. L. Freeouf, D. Shvydka, and A. D. Compaan, J. Appl. Phys. 85, 7418 (1999). E. A. Vinogradov, L. K. Vodop’yanov, and G. S. Oleinik, Sov. Phys. Solid State 15, 322 (1973). M. Gorska and W. Nazarewicz, Phys. Status Solidi B 65, 193 (1974). Z. C. Feng, P. Becla, L. S. Kim, S. Perkowitz, Y. P. Feng, H. C. Poon, K. P. Williams, and G. D. Pitt, J. Cryst. Growth 138, 239 (1994). M. Neumann-Spallart, E. Galun, G. Hodes, C. Levy-Clement, Y. Marfaing, E. Muranevich, and R. Tenne, J. Appl. Phys. 73, 7753 (1993). S. Cohen, R. Weil, and E. Muranevich, J. Appl. Phys. 76, 593 (1994). M. M. El-Nahass, A. A. M. Farag, and H. E. A. El-Sayed, Appl. Phys. A 77, 819 (2003). H. Okuyama, K. Nakano, T. Miyazima, and K. Akimoto, Jpn. J. Appl. Phys. 30, L1620 (1991). M. Ukita, H. Okuyama, M. Ozawa, A. Ishibashi, K. Akimoto, and Y. Mori, Appl. Phys. Lett. 63, 2082 (1993). U. Lunz, B. Jobst, S. Einfeldt, C. R. Becker, D. Hommel, and G. Landwehr, J. Appl. Phys. 77, 5377 (1995). U. Lunz, C. Schumacher, J. N€urnberger, K. Sch€ ull, A. Gerhard, U. Sch€ ussler, B. Jobst, W. Faschinger, and G. Landwehr, Semicond. Sci. Technol. 12, 970 (1997). K. Naniwae, H. Iwata, and K. Yashiki, Appl. Phys. Lett. 74, 3984 (1999). J. Wu, W. Walukiewicz, K. M. Yu, J. W. Ager III, W. Shan, E. E. Haller, I. Miotkowski, A. K. Ramdas, and S. Miotkowska, Appl. Phys. Lett. 80, 34 (2002). Y. Niiyama and M. Watanabe, Semicond. Sci. Technol. 20, 1187 (2005). V. Wagner, A. Fleszar, J. Geurts, G. Reusher, M. Keim, A. Waag, G. Landwehr, K. Wilmers, N. Esser, and W. Richter, J. Cryst. Growth 214/215, 340 (2000). A. A. Wronkowska, F. Firszt, H. Arwin, A. Wronkowski, M. Wakula, K. Strzalkowski, and W. Paszkowicz, Phys. Status Solidi C 3, 1193 (2006). T. Morita, H. Shinbo, H. Shinbo, T. Nagano, I. Nomura, A. Kikuchi, and K. Kishino, J. Appl. Phys. 81, 7575 (1997). S. P. Guo, O. Maksimov, M. C. Tamargo, F. C. Peiris, and J. K. Furdyna, Appl. Phys. Lett. 77, 4107 (2000). F. C. Peiris, J. K. Furdyna, S. P. Guo, and M. C. Tamargo, J. Appl. Phys. 89, 3748 (2001).

11 Elasto-optic, Electro-optic and Nonlinear Optical Properties 11.1 ELASTO-OPTIC EFFECT 11.1.1 Group-IV Semiconductor Alloy Data relating to elasto-optic behavior plays an important role not only in the design of elasto-optic devices, such as light modulators, deflectors and switches, but also in the analysis of lattice-mismatched semiconductor heterostructures. Photoelasticity is dependent on wavelength [1–4]. The photoelastic coefficient in 6H-SiC has been measured by Geidur [5]. Since the fundamental absorption edge of 6H-SiC is an indirect band gap, its contribution to the photoelasticity is negligibly small. Neither theoretical nor experimental studies relating to photoelasticity have been carried out on any group-IV semiconductor alloy.

11.1.2 III–V Semiconductor Alloy A method for calculating the photoelastic coefficients in III–V semiconductors has been described by Adachi and Oe [6]. This model was applied to AlxGa1xAs and GaxIn1xPyAs1y/ InP. The photoelastic coefficient ape for AlxGa1xAs under X||[100] stress has been reproduced in Figure 11.1. The black and gray circles correspond to the experimental data for GaAs (x ¼ 0) and Al0.5Ga0.5As, respectively. The definition of ape can be found in Adachi [1]. More recently, Kikkarin et al. [7] have calculated the spectral dependence of the photoelastic constants, p11, p12 and p44, for AlxGa1xAs with x up to 0.3. They also discussed the acousto-optic interaction in AlxGa1xAs/GaAs waveguides.

11.1.3 II–VI Semiconductor Alloy The photoelastic constants pij can be determined from the Brillouin scattering crosssections [1]. Ziobrowski et al. [8] used Brillouin scattering on BexZn1xSe and obtained pij at l ¼ 488 nm (0 x 0.25). Adachi and Hamaguchi [9] carried out resonant Brillouin scattering measurements on ZnxCd1xTe and obtained the spectral dependence of p44 for x ¼ 0.65 and 0.80. The data suggest that the sign for p44 in ZnxCd1xTe is negative in the region remote from the E0 edge and becomes positive when the wavelength approaches the band edge, as in ZnTe and CdTe [4].

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

358

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 11.1 Photoelastic coefficient ape for AlxGa1xAs with increments in x of 0.2. The black and gray circles correspond to the experimental data for GaAs (x ¼ 0) and Al0.5Ga0.5As, respectively. [Reprinted with permission from S. Adachi and K. Oe, J. Appl. Phys. 54, 6620 (1983). Copyright (1983), American Institute of Physics]

11.2 LINEAR ELECTRO-OPTIC CONSTANT 11.2.1 Group-IV Semiconductor Alloy Principally, the diamond lattice shows no linear electro-optic effect [1]. The linear electro-optic constant r41 for 3C-SiC has been reported to be 2.7 0.5 pm/Vat l ¼ 632.8 nm [10]. There is an ordered alloy phase in SixGe1x (Section 1.3.2) and this phase will exhibit a linear electrooptic effect [11], but no data are available at present.

11.2.2 III–V Semiconductor Alloy The linear electro-optic effect in AlxGa1xAs has been studied by Glick et al. [12]. They measured the electro-optic phase difference in an Al0.17Ga0.83As waveguide and determined r41 at l ¼ 1.1523 mm, as shown in Table 11.1. Bach et al. [13] have measured r41 for GaxIn1xPyAs1y/InP (y ¼ 0.20 and 0.34). The values they obtained are summarized in Table 11.1. Figure 11.2 also shows the theoretical r41 dispersion obtained by Adachi and Oe [14], together with the data produced by Bach et al. (y ¼ 0.34) [13]. It can be seen that the theoretical r41 curve shows strong dispersion near E0 (l 1.1 mm). This curve was obtained from an electric-field-induced modulation of the electronic energy-band structure.

11.2.3 II–VI Semiconductor Alloy The linear electro-optic constant r41 at l ¼ 1.5 mm of Bridgman-grown Zn0.1Cd0.9Te has been measured by Zappettini et al. [15] (see Table 11.1). The implementation of a Zn0.1Cd0.9Tebased electro-optic switch which reaches 30 dB of extinction ratio and sub millisecond response time has also been presented by the same authors.

ELASTO-OPTIC, ELECTRO-OPTIC AND NONLINEAR OPTICAL PROPERTIES

359

Table 11.1 Linear electro-optic constant r41 for some III–V and II–VI semiconductor alloys. S ¼ clamped value System

Alloy

x (y)

III–V

AlxGa1xAs

0 0.17 0.20 (y) 0.34 (y) 0.34 (y) 1.00 (y)

GaxIn1xPyAs1y/InP

II–VI

ZnxCd1xTe

0 0.1 1.0

r41 (pm/V)

l (mm)

Comments

1.80a 1.43b 1.34c 1.43c 1.44c 1.68a

10.6 1.1523 1.32 1.25 1.32 1.50

S

10.6 1.5 10.6

S (|r41|) S (|r41|) S (|r41|)

4.1a 4.3d 3.9a

S

S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors. John Wiley & Sons, Ltd, Chichester, 2005 M. Glick et al., J. Appl. Phys. 63, 5877 (1988) c H. G. Bach et al., Appl. Phys. Lett. 42, 692 (1983) d A. Zappettini et al., J. Electron. Mater. 30, 743 (2001) a b

Figure 11.2 Theoretical r41 and R11R12 curves along with the experimental data of Bach et al. [13] for GaxIn1xPyAs1y/InP with y ¼ 0.34. [Reprinted with permission from S. Adachi and K. Oe, J. Appl. Phys. 56, 1499 (1984). Copyright (1984), American Institute of Physics]

The electro-optic constants rij of w-CdSxSe1x have been measured by several authors [16,17]. The results obtained by Baldassarre et al. [16] are r13 ¼ 1.5 pm/Vand r33 ¼ 2.4 pm/V at l ¼ 632.8 nm for x ¼ 0.75. More recently, Bini and Razzetti [17] reported the unclamped electro-optic constant T rcT ¼ r13

3 no T r33 ne

ð11:1Þ

to be 5.81 0.03 pm/V for x ¼ 0.5, where no and ne are, respectively, the ordinary and extraordinary refractive indices and rijT is the unclamped electro-optic tensor component [14]. These authors also obtained rcT ¼ 6:45 0:03 pm=V for w-CdS and 7.23 0.04 pm/V for

360

PROPERTIES OF SEMICONDUCTOR ALLOYS

w-CdSe. A smaller alloy value than those of the endpoint binaries is considered to be due to the microscopic strains present in the alloy.

11.3 QUADRATIC ELECTRO-OPTIC CONSTANT 11.3.1 Group-IV Semiconductor Alloy No detailed data are available for group-IV semiconductor alloys.

11.3.2 III–V Semiconductor Alloy Bach et al. [13] have studied the quadratic electro-optic effect in GaxIn1xPyAs1y/InP double-heterostructure waveguides. They obtained the quadratic electro-optic constants R11 R12 ¼ 0.8 1020 m2/V2 at l ¼ 1.32 mm for y ¼ 0.20 and R11 R12 ¼ 5.8 1020 (3.1 1020) m2/V2 at l ¼ 1.25 (1.32) mm for y ¼ 0.35. These results (y ¼ 0.35) are shown in Figure 11.2, together with the theoretical R11 R12 values calculated by Adachi and Oe [18]. It can be seen that the quadratic electro-optic constant R11 R12 shows very strong dispersion compared with the linear electro-optic constant (r41).

11.3.3 II–VI Semiconductor Alloy No detailed data are available for II–VI semiconductor alloys.

11.4 FRANZ–KELDYSH EFFECT 11.4.1 Group-IV Semiconductor Alloy Although the Franz–Keldysh effect in the indirect absorption edge of SiC has been discussed [19], no detailed data are available for group-IV semiconductor alloys.

11.4.2 III–V Semiconductor Alloy To our knowledge, there have been no publications relating to the direct measurement of the absorption edge shift in AlxGa1xAs under an applied electric field. The Franz–Keldysh effect in GaxIn1xPyAs1y/InP has been studied experimentally by several authors [13,20–22]. The change in the optical absorption coefficient Da observed in InP/GaInPAs/InP p-i-n double heterostructures [22] is found to be comparable with that obtained from the quantum-confined Stark effect (103 cm1).

11.4.3 II–VI Semiconductor Alloy Samuel et al. [23] measured the absorption coefficients near the fundamental absorption edge of ZnxCd1xSe and CdSxSe1x. They found that most of the results can be explained by the Dow–Redfield theory of the internal Franz–Keldysh effect. An enhancement of the two-photon

ELASTO-OPTIC, ELECTRO-OPTIC AND NONLINEAR OPTICAL PROPERTIES

361

absorption coefficient has also been observed to occur in the space charge region of the CdxHg1xTe p-n junction, which can be attributed to the Franz–Keldysh effect induced by the built-in electric field [24].

11.5 NONLINEAR OPTICAL CONSTANT 11.5.1 Group-IV semiconductor alloy The independent non-vanishing tensor elements of the nonlinear optical constants for semiconductors of certain symmetry classes are given in [1]. Principally, the diamond lattice does not show a second-order nonlinear optical effect [1]. No detailed data are available on the third-order nonlinear optical constants for group-IV semiconductor alloys.

11.5.2 III–V semiconductor alloy The second-order nonlinear optical susceptibilities for w-AlxGa1xN with 0 x 0.666 have been measured by Sanford et al. [25]. These authors determined the nonlinear optical susceptibility constants d31 and d33 at l ¼ 1.064 mm as a function of x under the assumption of d31 ¼ d15. These results are shown in Figure 11.3(a), together with the endpoint data taken from Adachi [1]. The nonlinear susceptibility constant d31 decreases almost linearly with increasing x, while d33 largely scatters. The nonlinear optical susceptibility d14 at l ¼ 1.064 mm in AlxGa1xAs has been measured using a reflected second harmonics method by Ohashi et al. [26]. They reported the magnitudes of d14 relative to GaAs over the whole alloy range 0 x 1.0. These results are shown in Figure 11.3(b). The GaAs and AlAs d14 values in Adachi [3] are in the ranges 119–170 and 32 pm/V, respectively.

15

1.0

140

10

-10 -15 (a) w-AlxGa1-xN

-20 -25

0

0.2 0.4 0.6 0.8 1.0 x

100 d14 (pm/V)

d33

|d14(x)/d14(GaAs)|

d31, d33 (pm/V)

0 -5

120

0.8

d31

5

0.6 0.4

80 60 40

0.2 0

(b) AlxGa1-xAs 0

0.2 0.4 0.6 0.8 1.0 x

(c) ZnxCd1-xTe

20 0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 11.3 Second-order nonlinear optical susceptibility constants dij in (a) w-AlxGa1xN, (b) AlxGa1xAs and (c) ZnxCd1xTe. The experimental data in (a) are taken from Adachi [1] and Sanford et al. [25], in (b) from Ohashi et al. [26] and in (c) from Adachi [4] (open circles) and Zappettini et al. [31] (solid circles)

362

PROPERTIES OF SEMICONDUCTOR ALLOYS

The third-order nonlinear susceptibility |x (3)| in GaxIn1xPyAs1y/InP (lg 1.5 mm) has been determined using a forward degenerate four-wave mixing method [27]. The |x (3)| value obtained was 3.8 103 esu. The two-photon absorption coefficient b has been discussed both theoretically and experimentally for non-alloyed group-IV, III–Vand II–VI semiconductors [1]. Krishnamurthy et al. [28] showed that theoretically, b can be increased or decreased by adding In or Al to the GaN compound. Experimentally, Villeneuve et al. [29] obtained the spectral dependence of b near half the band gap of Al0.18Ga0.82As. The b increased with decreasing wavelength l (0.05 cm/GW at l ¼ 1.65 mm and 1.2 cm/GW at l 1.49 cm/GW). The three-photon absorption coefficient a in Al0.18Ga0.82As was also measured for photon energies between onehalf and one-third the band gap by Kang et al. [30]. They found that a decreases with decreasing l from a 0.13 cm3/GW2 at l ¼ 1.66 mm to a 0.03 cm3/GW2 at l ¼ 1.50 mm.

11.5.3 II–VI semiconductor alloy The second harmonic generation efficiency has been examined in the near-IR region (l ¼ 1.5 and 1.9 mm) of ZnxCd1xTe with x ¼ 0, 0.1, 0.2 and 1.0 [31]. The d14 data for ZnxCd1xTe [31], together with the endpoint data taken from Adachi [4], have been plotted in Figure 11.3(c). The solid line represents the linear least-squares fit given by d14 ¼ 73 13x pm/V. The second-order nonlinear constant d14 of CdxHg1xTe with x ¼ 0.277 has been determined to be 350 40 pm/V [32]. The second harmonic generation has also been measured at l ¼ 1.06 mm as a function of x for w-ZnxCd1xS and w-CdSxSe1x [33]. The two-photon absorption phenomena have been studied in several II–VI semiconductor alloys [34,35]. The maximum value of the two-photon absorption coefficient b is observed for x ¼ 0.4 in c-MgxZn1xSe (0 x 0.4) [34]. In c-ZnxCd1xSe and w-ZnxCd1xSe (0 x 1.0), the reduction in the band gap is accompanied by a smooth rise of b [35]. Tunability of the twophoton absorption coefficient has also been demonstrated by adjusting the electrical field in a CdxHg1xTe photodiode with a cutoff wavelength of 5.2 mm [24].

REFERENCES [1] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [2] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [3] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 2 III–V Compound Semiconductors, Kluwer Academic, Boston, 2004. [4] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 3 II–VI Compound Semiconductors, Kluwer Academic, Boston, 2004. [5] S. A. Geidur, Opt. Spectrosc. 49, 105 (1980). [6] S. Adachi and K. Oe, J. Appl. Phys. 54, 6620 (1983). [7] S. M. Kikkarin, D. V. Petrov, A. V. Tsarev, and I. B. Yakovkin, Proc. SPIE 1932, 234 (1993). [8] P. Ziobrowski, M. Drozdowski, M. Szybowicz, F. Firszt, S. Ł e˛ gowski, and H. Meczy ˛ nska, J. Appl. Phys. 93, 3805 (2003). [9] S. Adachi and C. Hamaguchi, J. Phys. Soc. Jpn 44, 343 (1978). [10] X. Tang, K. G. Irvine, D. Zhang, and M. G. Spencer, Appl. Phys. Lett. 59, 1938 (1991). [11] R. A. Soref, J. Appl. Phys. 72, 626 (1992).

ELASTO-OPTIC, ELECTRO-OPTIC AND NONLINEAR OPTICAL PROPERTIES [12] [13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34] [35]

363

M. Glick, F.-K. Reinhart, and D. Martin, J. Appl. Phys. 63, 5877 (1988). H. G. Bach, J. Krauser, H. P. Nolting, R. A. Logan, and F. K. Reinhart, Appl. Phys. Lett. 42, 692 (1983). S. Adachi and K. Oe, J. Appl. Phys. 56, 74 (1984). A. Zappettini, L. Cerati, A. Milani, S. M. Pietralunga, P. Boffi, and M. Martinelli, J. Electron. Mater. 30, 743 (2001). L. Baldassarre, A. Cingolani, and M. Sibilano, Opt. Commun. 26, 72 (1978). S. Bini and C. Razzetti, Phys. Status Solidi A 148, 603 (1995). S. Adachi and K. Oe, J. Appl. Phys. 56, 1499 (1984). R. G. Verenchikova and A. O. Konstantinov, Sov. Phys. Semicond. 18, 242 (1984). R. H. Kingston, Appl. Phys. Lett. 34, 744 (1979). K. Okamoto, S. Matsuoka, Y. Nishiwaki, and K. Yoshida, J. Appl. Phys. 56, 2595 (1984). B. Kn€upfer, P. Kiesel, A. H€ofler, P. Riel, G. H. D€ohler, and E. Veuhoff, Appl. Phys. Lett. 62, 2072 (1993). L. Samuel, Y. Brada, and R. Beserman, Phys. Rev. B 37, 4671 (1988). H. Y. Cui, Z. F. Li, Z. L. Liu, C. Wang, X. S. Chen, X. N. Hu, Z. H. Ye, and W. Lu, Appl Phys. Lett. 92, 021128 (2008). N. A. Sanford, A. V. Davydov, D. V. Tsvetkov, A. V. Dmitriev, S. Keller, U. K. Mishra, S. P. DenBaars, S. S. Park, J. Y. Han, and R. J. Molnar, J. Appl. Phys. 97, 053512 (2005). M. Ohashi, T. Kondo, R. Ito, S. Fukatsu, Y. Shiraki, K. Kumata, and S. S. Kano, J. Appl. Phys. 74, 596 (1993). M. N. Islam, E. P. Ippen, E. G. Burkhardt, and T. J. Bridges, J. Appl. Phys. 59, 2619 (1986). S. Krishnamurthy, K. Nashold, and A. Sher, Appl. Phys. Lett. 77, 355 (2000). A. Villeneuve, C. C. Yang, G. I. Stegeman, C.-H. Lin, and H.-H. Lin, Appl. Phys. Lett. 62, 2465 (1993). J. U. Kang, A. Villeneuve, M. Sheik-Bahae, G. I. Stegeman, K. Al-hemyari, J. S. Aitchison, and C. N. Ironside, Appl. Phys. Lett. 65, 147 (1994). A. Zappettini, S. M. Pietralunga, A. Milani, D. Piccinin, M. Fere, and M. Martinelli, J. Electron. Mater. 30, 738 (2001). A. W. Wark, D. Pugh, L. E. A. Berlouis, and F. R. Cruickshank, J. Appl. Phys. 89, 306 (2001). R. A. Soref and H. W. Moos, J. Appl. Phys. 35, 2152 (1964). B. Derkowska, B. Sahraoui, X. N. Phu, G. Glowacki, and W. Bala, Opt. Mater. 15, 199 (2000). M. S. Brodin and D. B. Goer, Sov. Phys. Semicond. 5, 219 (1971).

12 Carrier Transport Properties 12.1 INTRODUCTORY REMARKS The electrical resistivity r, together with the thermal resistivity W, for CuxAu1x is shown in Figure 12.1. The solid and open circles correspond to the ordered (CuAu and Cu3Au) and disordered alloys, respectively. The experimental data are taken from various sources. The W data plots in Figure 12.1(b) are the same as those in Figure 2.24. The solid and dashed lines in Figure 12.1(a) are calculated from Equation (A.17) with CCuAu ¼ 60 mW cm and with and without properly taking into account the effect of alloy ordering at x ¼ 0.5 and 0.75 (CuAu and Cu3Au), respectively. As mentioned in Section 2.5.1, the Wiedemann–Franz law states that the ratio of the thermal conductivity K (¼W1) to the electrical conductivity s (¼r1) is proportional to the temperature. Thus, at any temperature s (r) is proportional to K (W), as can be seen in Figure 12.1. In semiconductor alloys, the potential fluctuations of electrons are a result of the compositional disorder. This effect produces a peculiar scattering mechanism, namely, alloy scattering. Alloy-scattering-limited mobility is represented as [1] mal e

pﬃﬃﬃﬃﬃﬃ 2p e h4 Nal ¼ 3 ðkTÞ1=2 ðme Þ5=2 xð1xÞðDUe Þ2

ð12:1Þ

where me is the electron effective mass, Nal is the density of alloy sites, DUe is the alloy scattering potential and x and (1 x) are the mole fractions of the endpoint materials. The alloy scattering mechanism shown in Equation (12.1) leads to a decrease in the electron mobility me at x „ 0 or 1.0. Not only the electrons but also the holes are subject to potential fluctuations as a result of the compositional disorder. Alloy scattering may, therefore, be observable both in n- and p-type 5=2 semiconductor alloys. However, because of its mass dependence (i.e. me;h ), the scattering strength may be weaker in p-type alloys than in n-types. The electron and hole Hall mobilities (me and mh) measured at room temperature for a number of non-alloyed group-IV, III–V and II–VI semiconductors are summarized in Table 12.1. These values, together with the bowing parameters ce and ch listed in Table 12.2, can be used for obtaining the mobilities of alloys of arbitrary composition. Electron and hole saturation drift velocities, minority carrier lifetimes and impact ionization coefficients for some non-alloyed group-IV, III–V and II–VI semiconductors can be found in Adachi [2].

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

366

PROPERTIES OF SEMICONDUCTOR ALLOYS 20

3 (a)

(b)

CuxAu1-x

W (cmK/W)

ρ (μΩ cm)

15

10

2

1

5 CuAu Cu3Au

0 0

0.2 0.4 0.6 0.8 1.0 x

CuAu Cu3Au

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.1 Electrical r and thermal resistivities W for CuxAu1x at 300 K. The theoretical curves are obtained from Equation (A.17) (Equation (2.25)) with CCuAu ¼ 60 mW cm (r) and 8.15 cm K/W (W) and with (solid lines) and without properly taking into account the alloy ordering effect at x ¼ 0.5 and 0.75 (CuAu and Cu3Au) (dashed lines), respectively

Table 12.1 Room-temperature electron and hole Hall mobilities me and mh for some cubic and hexagonal semiconductors. d ¼ diamond, zb ¼ zinc-blende, h ¼ hexagonal, w ¼ wurtzite, rs ¼ rocksalt System Material IV

III–V

a

me (cm2/V s) mh (cm2/V s) System Material

Diamond (d) Si (d) Ge (d) 3C-SiC (zb) 6H-SiC (h) BP (zb) AlN (w) AlP (zb) AlAs (zb) AlSb (zb) GaN (zb) GaN (w) GaP (zb) GaAs (zb) GaSb (zb) InN (w) InP (zb) InAs (zb) InSb (zb)

2800 1750a 4330 980 375 190 125 80 294 200 760 1245 189 9340 12040 3100 6460 33000 77000

Drift (conductivity) mobility

1500 480 2400 60 100 500 14 450 105 420 350 370 140 450 1000 39 180 450 1100

II–VI MgO (rs) ZnO (w) ZnS (zb) ZnS (w) ZnSe (zb) ZnTe (zb) CdO (rs) CdS (zb) CdS (w) CdSe (w) CdTe (zb) HgS (zb) HgSe (zb) HgTe (zb)

me (cm2/V s) mh (cm2/V s) 440 275 140 1500 600 216 85 390 900 1260a 230 22000 32000

10 267 72 355 100 48 50 104 320

CARRIER TRANSPORT PROPERTIES

367

Table 12.2 Bowing parameters ce and ch for the electron and hole mobilities me and mh in some group-IV binaries, and III–V and II–VI ternaries System IV III–V

Alloy CxSi1x SixGe1x w-AlxGa1xN GaxIn1xP AlxGa1xAs AlxIn1xAs GaxIn1xAs AlxGa1xSb GaxIn1xSb GaPxSb1x GaAsxSb1x InPxAs1x InPxSb1x InAsxSb1x

ce (cm2/V s) ch (cm2/V s) System 5200 11000 900 18000 35000 26000 42000 20000 30000 110000 30000

3600 2200

IIVI

40 520

Alloy CdxHg1xSe ZnxCd1xTe c-ZnSxSe1x ZnSexTe1x

ce (cm2/V s) ch (cm2/V s) 30000 2800 3200

160

600 2500 1000 2500

12.2 LOW-FIELD MOBILITY 12.2.1 Group-IV Semiconductor Alloy (a) CSi binary alloy The electron and hole mobilities me and mh for Si (x ¼ 0), diamond (x ¼ 1.0) and 3C-SiC (x ¼ 0.5), respectively are shown in Figure 12.2(a). The solid lines represent the quadratic fits of Equation (A.17) with ce,h in Table 12.2. Note that 3C-SiC is an ordered form of CxSi1x, or in other words, a compound. We can, thus, expect no alloy scattering in 3C-SiC. However, the 3CSiC mobilities are smaller than the mean values of diamond and Si, especially for mh. The lower 3C-SiC values may be due to its poorer crystalline quality. (b) SiGe binary alloy Figure 12.2(b) shows the electron and hole mobilities me and mh for SixGe1x. It is obvious that not only is alloy scattering, but also that the other scattering mechanisms and the effective masses modified through the change of the band structure influence the electron mobility in this alloy. The mass and temperature dependence of each scattering mechanism 5=2 is summarized in Table 12.2 of Adachi [2], including alloy scattering (m / me;h , m/T1/2). The most prominent example is the decrease in me at x 0.15, which corresponds to the transition from a Ge-like CB (L) to a Si-like CB (X or D) (Figure 6.8). The main effect on me is, thus, associated with the increase in the electron conductivity mass in the Si-like CB for x 0.15 (Figure 7.3). For SixGe1x, mh was not found to be strongly dependent on x.

368

PROPERTIES OF SEMICONDUCTOR ALLOYS

μe (103 cm2/Vs)

5 4

5

(a) Cx Si1-x

Ge-like CB

3

3 3C-SiC

2

2

1

1

0

0

2.0

μh (103 cm2/Vs)

(b) SixGe1-x

4

1.5

3.0

(a) CxSi1-x

2.0

1.0

1.5 1.0

3C-SiC

0.5 0 0

(b) SixGe1-x

2.5

0.5 0.2

0.4

0.6

0.8

1.0

0 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 12.2 Electron and hole mobilities me and mh for (a) CxSi1x and (b) SixGe1x at 300 K. The solid lines show the calculated results using Equation (A.17) and the numeric parameters in Tables 12.1 and 12.2

12.2.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N alloy The electron mobility me for some (III, III)–V ternary alloys, w-AlxGa1xN, w-AlxIn1xN and w-GaxIn1xN, plotted against x is shown in Figure 12.3. The me values for w-AlxGa1xN can be expressed by Equation (A.5) with ce ¼ 900 cm2/V s (Table 12.2). No large me values have been obtained for w-AlxIn1xN and w-GaxIn1xN ternaries. Very weak temperature dependence of 1.5

4 (a) w-AlxGa1-xN

μe (103 cm2/Vs)

1.2

4 (b) w-AlxIn1-xN

1.0 (c) w-GaxIn1-xN

3

3

2

2

0.9

0.6

0.6

0.4 1

0.3 0

(d) AlxGa0.98-xIn0.02N

0.8

0 0.2 0.4 0.6 0.8 1.0 x

0

1

0 0.2 0.4 0.6 0.8 1.0 x

0

0.2

0 0.2 0.4 0.6 0.8 1.0 x

0 0 0.2 0.4 0.6 0.8 1.0 x

Figure 12.3 Electron mobility me for (a) w-AlxGa1xN, (b) w-AlxIn1xN, (c) w-GaxIn1xN and (d) w-AlxGa0.98xIn0.02N at 300 K. The solid line in (a) shows the result calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

CARRIER TRANSPORT PROPERTIES

369

the free-electron density in w-GaxIn1xN with In-rich compositions (x 0.08) [3] suggests that the materials are metallic-like. (b) (III, III)–P alloy The electron and hole mobilities for GaxIn1xP are shown in Figure 12.4. Some data correspond to those for GaxIn1xP lattice-matched to GaAs. The lowest CB in InP (x ¼ 0) is located at the G point, while that in GaP is at the X point. The large (small) me value for InP (GaP) is principally due to the small (large) electron effective mass in the G (X) valley, as shown in Figure 12.4(a) by the open circles. There is a clear relationship between the electron effective mass mac (or mGe ) and electron mobility me. We can estimate from Equations (12.19) and (12.21) in Adachi [2] the X- and G-valley electron mobilities to be 220 (InP) and 990 cm2/V s (GaP), respectively. These values are plotted in Figure 12.4(a) by the open triangles. 8

2.5 (a)

(b)

2.0 Γ-valley

μh (102 cm2/Vs)

μe (103 cm2/Vs)

6

4

2 X-valley

0 0

0.2 0.4 0.6 0.8 1.0 x

1.5 1.0 0.5 0 0

GaxIn1-xP 0.2 0.4 0.6 0.8 1.0 x

Figure 12.4 Electron and hole mobilities me and mh for GaxIn1xP at 300 K. The solid line in (b) shows the result calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

(c) (III, III)–As alloy The electron and hole mobilities for some (III, III)As ternaries are plotted in Figure 12.5. The AlxGa1xAs and AlxIn1xAs ternaries show the G X crossover at x 0.4 and 0.6, respectively (Figures 6.20 and 6.22). These alloys may, thus, provide an abrupt change in me at such crossover points due to the different effective masses at the G and X valleys. From Equations (12.19) and (12.21) in Adachi [2], we can estimate the X- and G-valley electron mobilities to be 330 (GaAs) and 830 cm2/V s (AlAs), respectively. These values are also shown in Figure 12.5(a) by the open triangles. Similarly, we can estimate the X-valley electron mobility to be 270 cm2/V s, as plotted in Figure 12.5(b) by the open triangle (InAs). The G-electron bowing parameters for me and those for mh are listed in Table 12.2. The low-field transport properties of AlxGa1xAs have also been reviewed in more detail in Adachi [1]. (d) (III, III)–Sb alloy The electron and hole mobilities for some (III, III)–Sb ternaries are plotted in Figure 12.6. Like (Al, III)–As in Figure 12.5, the AlxGa1xSb and AlxIn1xSb alloys show the G X crossover at

370

PROPERTIES OF SEMICONDUCTOR ALLOYS

μh (102 cm2/Vs)

μe (104 cm2/Vs)

1.2

4

4

(a) AlxGa1-xAs

(b) AlxIn1-xAs

0.9

(c) GaxIn1-xAs

3 Γ-valley

0.6

Γ-valley

2

0.3

2

1

X-valley

0

0

5

5

(a) AlxGa1-xAs

4

3

1

X-valley

0 5

(b) AlxIn1-xAs

4

3

3

3

2

2

2

1

1

1

0

0

0.2

0.4

0.6

0.8

1.0

0

0

0.2

0.4

x

0.6

(c) GaxIn1-xAs

4

0.8

0 1.0 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 12.5 Electron and hole mobilities me and mh for (a) AlxGa1xAs, (b) AlxIn1xAs and (c) GaxIn1xAs at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

μh (103 cm2/Vs)

μe (104 cm2/Vs)

2.0

10

(a) AlxGa1-xSb 1.5 Γ-valley

1.0

8

10

(b) AlxIn1-xSb Γ-valley

6

6

4

4

0.5

2

2

0 1.5

0

0

1.5

2.0

X-valley

(a) Al xGa1-xSb

(c) Ga xIn1-xSb

8

(b) AlxIn1-xSb

1.0

1.0

0.5

0.5

(c) GaxIn1-xSb 1.5 1.0

0

0

0.2

0.4

0.6 x

0.8

1.0 0 0

0.5 0.2

0.4

0.6 x

0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 12.6 Electron and hole mobilities me and mh for (a) AlxGa1xSb, (b) AlxIn1xSb and (c) GaxIn1xSb at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

x 0.5 and 0.7, respectively (Figures 6.25 and 6.26). We can, thus, expect an abrupt change in me at such crossover points, although no enough experimental data are available. The dependence of me on x in GaxIn1xSb can be successfully explained using ce ¼ 42000 cm2/ V s (Table 12.2).

CARRIER TRANSPORT PROPERTIES

371

(e) Dilute-nitride III–(V, V) alloy The electron mobility should be lower in dilute-nitride III–V alloys due to strong carrier scattering and enhanced electron effective masses [4,5]. The experimental mobility me for dilutenitrideGaNxAs1x andInNxAs1x ternariesisshowninFigure12.7.Itcanbeseenthattheaddition of small concentrations of N to GaAs or InAs leads to a large reduction in me. The reduction in me determined experimentally seemed to be larger than that predicted theoretically [4,5]. 105

105

(b) InNxAs1-x

104

μe (cm2/Vs)

μe (cm2/Vs)

(a) GaN xAs1-x

103

102 0

1

2 3 x (at%)

4

104

103

102 0

1

2 3 x (at%)

4

Figure 12.7 Electron mobility me for (a) dilute-nitride GaNxAs1x and (b) dilute-nitride InNxAs1x at 300 K. The open circles show the endpoint binary data taken from Table 12.1

Since the VB of the III–V semiconductors is mainly characterized by the electron orbital of the group V anions [2], we can expect that N addition will not have a strong effect on the hole mobility. However, the experimental mh value dramatically decreased from 300 cm2/V s at x ¼ 0 at% (GaAs) to 80 cm2/V s at x ¼ 1 at% [6]. This drop in mh is likely correlated with the increase in crystalline defects introduced by nitrogen doping. (f) Ga–(V, V) alloy Figure 12.8 shows the electron and hole mobilities for some Ga–(V, V) ternary alloys. As in AlxGa1xAs, the CB in GaPxAs1x shows the G X crossover at x ¼ 0.48 (Figures 6.33). GaPxAs1x, thus, shows an abrupt change in me near x ¼ 0.48. The open triangles in Figures 12.8 (a) and 12.8(b) plot the X- and G-valley electron mobilities for GaAs (GaSb) and GaP as estimated from Equations (12.19) and (12.21) in Adachi [2], respectively. (g) In–(V, V) alloy The experimental electron mobility for some In–(V, V) ternaries have been plotted in Figure 12.9. The solid lines represent the me versus x curves calculated from Equation (A.5) with ce taken from Table 12.2.

12.2.3 III–V Semiconductor Quaternary Alloy (a) Dilute-nitride alloy The free-electron concentration and mobility have been found to be significantly reduced by the incorporation of N into Si-doped dilute-nitride GaxIn1xNyP1y [7] and GaxIn1xNyAs1y [8,9].

372

PROPERTIES OF SEMICONDUCTOR ALLOYS

μe (103 cm2/Vs)

10

15

(a) GaPxAs1-x

8

12

Γ-valley

6

15

(b) GaPxSb1-x

9

4 X-valley

6 Γ-valley

3

0

X-valley

3

0

1.2

0

1.2

1.2

(a) GaPxAs1-x

(b) GaPxSb1-x

(c) GaAsxSb1-x

0.9

0.9

0.9

0.6

0.6

0.6

0.3

0.3

0.3

0

0

0.2

0.4

0.6

0.8

(c) GaAsxSb1-x

9

6

2

μh (103 cm2/Vs)

12

0 1.0 0

0.2

x

0.4

0.6

0.8

0 1.0 0

0.2

0.4

x

0.6

0.8

1.0

x

Figure 12.8 Electron and hole mobilities me and mh for (a) GaPxAs1x, (b) GaPxSb1x and (c) GaAsxSb1x at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

4

10

10

(a) InPx As1-x

μ e (10 4 cm 2 /Vs)

3

(b) InPx Sb1-x

(c) InAsx Sb1-x

8

8

6

6

4

4

2

2

2

1

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

0

0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.9 Electron mobility me for (a) InPxAs1x, (b) InPxSb1x and (c) InAsxSb1x at 300 K. The solid lines show the results calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

No significant effect of N incorporation has, however, been observed on the hole transport properties of Be-doped GaxIn1xNyAs1y [9] and Zn-doped GaNxAs1xSb1xy [10]. (b) (III, III)–(V, V) alloy The variation in me and mh with y for GaxIn1xPyAs1y/InP is shown in Figure 12.10. The solid lines represent the quadratic expressions given by (in cm2/V s)

CARRIER TRANSPORT PROPERTIES 1.8

2.5

(a)

(b)

1.5

2.0

1.2

μ h (10 2 cm2 /Vs)

μ e (10 4 cm2 /V s)

GaxIn1-xPyAs1-y/InP

0.9 0.6

1.5

1.0

0.5

0.3 0

373

0

0.2

0.4

0.6

0.8

1.0

0 0

0.2

0.4

y

0.6

0.8

1.0

y

Figure 12.10 Electron and hole mobilities me and mh for GaxIn1xPyAs1y/InP at 300 K. The solid lines show the results calculated using Equation (12.2)

me ðyÞ ¼ 1520030740y þ 22000y2

ð12:2aÞ

mh ðyÞ ¼ 183383y þ 380y2

ð12:2bÞ

As can be seen in Figure 12.10, alloy scattering produces a mobility minimum at y 0.7 and 0.5 for me and mh, respectively. The low-field transport properties of GaxIn1xPyAs1y/InP have also been reviewed in more detail in Adachi [11]. (c) (III, III, III)–V alloy The electron mobility me versus x for w-AlxGa0.98xIn0.02N [12] has been plotted in Figure 12.3(d). As in w-AlxGa1xN (Figure 12.3(a)), me for w-AlxGa0.98xIn0.02N greatly decreases with increasing x. The electron mobility me as a function of x for (AlxGa1x)0.53In0.47P/GaAs and (AlxGa1x)0.48In0.52As/InP is plotted in Figures 12.11(a) and 12.11(b), respectively. The solid lines in Figures 12.11(a) and 12.11(b) show, respectively, the quadratic expressions given by (in cm2/V s) me ðxÞ ¼ 43006000x þ 3000x2

ð12:3aÞ

me ðxÞ ¼ 1520038400x þ 32000x2

ð12:3bÞ

The experimental data in Figure 12.11(a) are taken from Sotoodeh et al. [13] (open circle) and Hofmann et al. [14] (solid circles). The CB in (AlxGa1x)0.53In0.47P/GaAs shows the G X crossover at x 0.64 (Figure 6.49). Thus, the experimental me data for x > 0.64 in Figure 12.11 (a) seem to be questionably large.

374

PROPERTIES OF SEMICONDUCTOR ALLOYS 6

2.0

(a)

(b)

4 X-valley

3 2

(AlxGa1-x)0.48In0.52As/InP

1.5

μe (104 cm2/Vs)

μe (103 cm2/Vs)

5 (Al Ga ) In P/GaAs x 1-x 0.53 0.47

1.0

0.5

Γ-valley

1 0

0

0.2

0.4

0.6

0.8

0 0

1.0

x

0.2

0.4

0.6

0.8

1.0

x

Figure 12.11 Electron mobility me for (a) (AlxGa1x)0.53In0.47P/GaAs and (b) (AlxGa1x)0.48In0.52As/ InP at 300 K. The solid lines show the calculated results using Equation (12.3)

12.2.4 II–VI Semiconductor Alloy (a) (II, II)–O ternary alloy The large band-gap alloy MgxZn1xO is the subject of growing interest in connection with the development of UV optoelectronic devices based on ZnO. The low-field hole mobility mh is plotted against x for MgxZn1xO in Figure 12.12(a). The x ¼ 0.2 data provides the highest alloy mh value of 6.42 cm2/V s [15]. 103

2.5

(a) Mgx Zn1-xO

μh(cm /Vs) 2

mixed phase wurtzite rocksalt

100

10-1 0

μe (104 cm2/Vs)

2.0

102

101

(b) Cdx Hg1-xSe

1.5 1.0

zinc-blende wurtzite mixed phase

0.5

0.2 0.4 0.6 0.8 1.0 x

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.12 Electron mobility me for (a) MgxZn1xO and (b) CdxHg1xSe at 300 K. The solid line in (b) shows the results calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

(b) (II, II)–Se ternary alloy The electron Hall mobility for Bridgman-grown MgxZn1xSe (x 0.07) and MgxCd1xSe (x 0.4) has been measured at T ¼ 11300 K [16]. The me values for MgxZn1xSe

CARRIER TRANSPORT PROPERTIES

375

(MgxCd1xSe) with x ¼ 0.07 (0.4) are 225 (100) and 20 (0.2) cm2/V s at 300 and 11 K, respectively. The very low me values observed at low temperatures were considered to be due to the conduction at the impurity band. The electron mobility me for Bridgman-grown Fe-doped ZnxHg1xSe with x 0.072 has been measured in the temperature range 1.7–300 K [17]. The electron mobility for CdxHg1xSe has also been measured by several authors. The experimental data for CdxHg1xSe are shown in Figure 12.12(b). The solid line represents the dependence of me on x using Equation (A.5) with the numeric parameters shown in Tables 12.1 and 12.2. (c) (II, II)–Te ternary alloy Figure 12.13 shows the electron Hall mobility me for some (II, II)–Te ternaries. The hole Hall mobility mh for ZnxCd1xTe is also plotted in the lower part of Figure 12.13. Because ZnxCd1xTe is one of the most promising materials for use in room-temperature nuclear detectors, the carrier drift mobilities were usually measured in conjunction with the value of the mt (drift mobility–lifetime) product. Note that the solid triangles (me) in Figure 12.13(b) correspond to the electron drift mobility, not the Hall mobility. The highest me value for CdTe (x ¼ 0) reported so far is 1260 cm2/V s [18], which is considerably smaller than that predicted from the dashed line in Figure 12.13(b) (1600 cm2/V s).

μe (103 cm2/Vs)

1.2 0.9

3

(b) Zn xCd1-xTe 2

40 30

1

0.3

0.4

0.6

10 0.8

0

1.0 0 1.2

μh (102 cm2/Vs)

x

(c) Cd x Hg1-xTe

20

Γ-valley

0.2

semimetal

50

Hall mobility Drift mobility

X-valley

0.6

0 0

60

(a) Mg xCd1-xTe

0.2

0.4

0.6

0.8

1.0

0

0

0.2

0.4

0.6

0.8

1.0

x

(b) ZnxCd1-xTe

0.9 0.6 0.3 0

0

0.2

0.4

0.6

0.8

1.0

x

Figure 12.13 Electron and hole Hall mobilities me and mh for (a) MgxCd1xTe, (b) ZnxCd1xTe and (c) CdxHg1xTe at 300 K. The electron drift mobilities are also shown by the solid triangles in (b). The solid line in (b) shows the result calculated using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

As seen in Figure 12.13(c), the electron Hall mobility for CdxHg1xTe increases monotonically from x ¼ 0 to a peak at the semiconductorsemimetal transition x 0.08 with a peak mobility of 44000 cm2/V s and then drops monotonically with further increase in x. The lowfield electron and hole transport properties of CdxHg1xTe have been reviewed in more detail in Miles [19].

376

PROPERTIES OF SEMICONDUCTOR ALLOYS

(d) Zn–(V, V) ternary alloy The electronHall mobility forc-ZnSxSe1x and ZnSexTe1x ternaries is shown in Figures 12.14(a) and 12.14(b), respectively. The limited data predict that these alloys have considerably large bowing parameters ce, as listed in Table 12.2. 1.8

1.8

(b) ZnSe xTe1-x

1.5

1.5

1.2

1.2

μe (103 cm2/Vs)

μe (103 cm2/Vs)

(a) c-ZnS xSe1-x

0.9 0.6 0.3 0

0.9 0.6 0.3

0

0.2 0.4 0.6 0.8 1.0 x

0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.14 Electron mobility me for (a) c-ZnSxSe1x and (b) ZnSexTe1x at 300 K. The solid lines show the calculated results using Equation (A.5) and the numeric parameters in Tables 12.1 and 12.2

12.3 HIGH-FIELD TRANSPORT 12.3.1 Group-IV Semiconductor Alloy No detailed studies concerning the high-field transport properties of group-IV semiconductor alloys have been reported.

12.3.2 III–V Semiconductor Ternary Alloy (a) (III, III)–N alloy The high-field transport phenomena in AlxGa1xN and GaxIn1xN have been investigated using Monte Carlo simulation [20,21]. The electron drift velocity–field (ve E) characteristics obtained from these studies are summarized in Figure 12.15. The electron velocity at high fields tends to level off and is defined as the saturation velocity ve,sat. (b) (III, III)–P alloy The high-field transport properties of Ga0.5In0.5P/GaAs have been studied by several authors. Sakamoto et al. [22] determined the ve E curve for E up to 20 kV/cm at 300 K. Yee et al. [23] reported the temperature-dependent ve,sat up to 200 C by analyzing Ga0.5In0.5P/GaAs HBT characteristics. These results are shown in Figure 12.16. The electron drift velocity peaks at E 15 kV/cm with a value of vp 1.0 107 cm/s.

CARRIER TRANSPORT PROPERTIES

377

v Ep vp vsat 3.0

E

6 (a)

1.8 (b)

(c)

5 Ep (105 V/cm)

2.0

1.5

1.0 0

ve, sat (107 cm/s)

1.6

vp (107 cm/s)

2.5 4 3

1.4

2

1.2

AlxGa1-xN GaxIn1-xN

1

0.2 0.4 0.6 0.8 1.0 x

0 0

0.2 0.4 0.6 0.8 1.0 x

1.0 0

0.2 0.4 0.6 0.8 1.0 x

Figure 12.15 (a) Peak electron drift velocity vp, (b) peak field Ep and (c) electron saturation velocity ve,sat for AlxGa1xN and GaxIn1xN obtained using the Monte Carlo simulation at 300 K

12

6

ve, sat (106 cm/s)

10 ve (106 cm/s)

Ga0.5In0.5P/GaAs

(a)

8 6 4

5 4 3

2 0

(b) 0

5

10 15 E (kV/cm)

20

2

0

50 100 150 200 250 T (°C)

Figure 12.16 (a) Electron drift velocity versus field curve and (b) electron saturation velocity as a function of temperature for Ga0.5In0.5P/GaAs at 300 K. The experimental data in (a) are taken from Sakamoto et al. [22] and in (b) from Yee et al. [23]

(c) (III, III)–As alloy The veE curves for AlxGa1xAs have been determined using a pump-probe technique and transferred-electron devices [24]. As can be seen in Figure 12.17(a), the electron drift velocity at any fixed field decreases with increasing x. The hole drift velocity versus field (vh E) curves for Al0.45Ga0.55As have also been studied using an ensemble Monte Carlo technique [25]. These results, together with the experimental vh E curve for GaAs, are shown in the lower part of Figure 12.17(a).

378

PROPERTIES OF SEMICONDUCTOR ALLOYS

Figure 12.17 Electron and hole velocities versus filed curves for (a) AlxGa1xAs and (b) GaxIn1xAs. The data plotted in (a) are taken from Bhattacharya et al. [24] (ve E) and Brennan and Hess [25] (vh E, Monte Carlo simulation) and in (b) from Balynas et al. [26] (ve E) and Adachi [11] (vh E)

Figure 12.17(b) plots the ve,h E curves for Ga0.47In0.53As/InP [11,26]. We also show in the lower part of Figure 12.17(b) the experimental and calculated vh E curves for GaAs and InP, respectively. The hole velocity saturation in these materials occurs at fields of about 100 kV/cm, which are much higher than those for the electrons ( b [78,84]. The a and b coefficients for strained Ga0.2In0.8As have also been measured by fabricating lateral p-i-n diodes [85]. The results indicate that both a and b are larger than those for GaAs and furthermore b is larger than a. (d) (III, III)–Sb alloy Hildebrand et al. [86] reported resonance enhancement of b in a low field region for AlxGa1xSb with x ¼ 0.065 where E0 is equal to D0 (Figure 6.25). The b/a ratio exceeded 20. Zhingarev et al. [87] also measured a, b and their ratio for AlxGa1xSb (x ¼ 00.23). Kuwatsuka et al. [88] observed no strong enhancement of b/a in AlxGa1xSb near x ¼ 0.06. The b/a ratio obtained by Kuwatsuka et al. was 5 at the low electric field of 1.6 105 V/cm. More recently, Gouskov et al. [89] studied the impact ionization phenomena in AlxGa1xSb at x ¼ 0, 0.04 and 0.08 and obtained a maximum b/a at x ¼ 0.04. Theoretically, Rmou et al. [90] showed that if the alloy disorder in AlxGa1xSb is neglected, b exhibits a continuous variation with D0/E0; if not, b is strongly increased and shows a maximum at x ¼ 0.02. (e) Dilute-nitride III–(V, V) alloy A p-i-n avalanche photodiode using GaNxAs1x/GaAs was demonstrated [91]. The b/a ratio obtained was 0.4.

CARRIER TRANSPORT PROPERTIES

385

(f) Ga–(V, V) alloy The a and b values were determined for GaAsxSb1x (x ¼ 0.875 and 0.90) at 77 and 300 K [92]. The b/a ratios reported were 0.3 at 300 K (x ¼ 0.875), 0.4 at 77 K and 0.6 at 300 K (x ¼ 0.90). (g) In–(V, V) alloy The impact ionization coefficients for InAs0.12Sb0.88 were investigated and it was found that b is about 5 times larger than a in the field E ¼ (4 6) 104 V/cm [93].

12.5.3 III–V Semiconductor Quaternary Alloy (a) (III, III)–(V, V) alloy The a and b values at high electric fields ( > 180 kV/cm) for GaxIn1xPyAs1y/InP have been determined by Osaka et al. [94,95]. The b/a ratio versus y for GaxIn1xPyAs1y/InP [95] is reproduced in Figure 12.23. The ratio was found to increase with increasing y and to become unity, a ¼ b, at y 0.6. 101

β/α

GaxIn1-xPyAs1-y/InP 100

10-1 0

0.2

0.4

0.6

0.8

1.0

y

Figure 12.23 b/a ratio for GaxIn1xPyAs1y/InP. The experimental data are taken from Osaka et al. [95]

As in Ga0.47In0.53As, anomalous low-field behavior of a was observed in GaxIn1xPyAs1y/ InP [96]. No anomaly for b was observed in this quaternary [97]. The impact ionization phenomena in Ga0.80In0.20As0.17Sb0.83/GaSb have been studied by fabricating mesa photodiodes [98]. The a and b values in Equation (12.4) have been determined to be A ¼ 2.41 106 cm1 and B ¼ 4.45 105 V/cm with m ¼ 2.0 (a) and A ¼ 1.98 106 cm1 and B ¼ 3.69 105 V/cm with m ¼ 2.0 (b), respectively. The resulting b/a ratio is 47. (b) (III, III, III)–V alloy The parameterized a and b values in Equation (12.4) have been determined for Al0.24Ga0.24 In0.53As/InP to be A ¼ 2.29 107 cm1 and B ¼ 3.59 106 V/cm with m ¼ 1.0 (a) and A ¼ 1.42 107 cm1 and B ¼ 3.73 106 V/cm with m ¼ 1.0 (b), respectively (E ¼ 400–500 kV/cm) [99]. The relationship a > b can be predicted from these parameters. The impact ionization coefficients a and b for a strained Al0.22Ga0.63In0.15As layer grown on Al0.3Ga0.7 As/GaAs by MBE have also been determined by fabricating lateral p-i-n diodes [85].

386

PROPERTIES OF SEMICONDUCTOR ALLOYS

12.5.4 II–VI Semiconductor Alloy Although Brennan and Mansour [100] calculated the electron impact ionization coefficient for CdxHg1xTe, no detailed experimental data are available for II–VI semiconductor alloys.

REFERENCES [1] S. Adachi, GaAs and Related Materials: Bulk Semiconducting and Superlattice Properties, World Scientific, Singapore, 1994. [2] S. Adachi, Properties of Group-IV, III–V and II–VI Semiconductors, John Wiley & Sons, Ltd, Chichester, 2005. [3] S. -K. Lin, K. -T. Wu, C. -P. Huang, C. -T. Liang, Y. H. Chang, Y. F. Chen, P. H. Chang, N. C. Chen, C. A. Chang, H. C. Peng, C. F. Shih, K. S. Liu, and T. Y. Lin, J. Appl. Phys. 97, 046101 (2005). [4] M. P. Vaughan and B. K. Ridley, Phys. Rev. B 72, 075211 (2005). [5] S. Fahy, A. Lindsay, H. Ouerdane, E. P. OReilly, Phys. Rev. B 74, 035203 (2006). [6] A. J. Ptak, S. W. Johnston, S. Kurtz, D. J. Friedman, and W. K. Metzger, J. Cryst. Growth 251, 392 (2003). [7] Y. G. Hong, A. Nishikawa, and C. W. Tu, Appl. Phys. Lett. 83, 5446 (2003). [8] Y. -S. Kang, L. H. Robins, A. G. Birdwell, A. J. Shapiro, W. R. Thurber, M. D. Vaudin, M. M. E. Fahmi, D. Bryson, and S. N. Mohammad, J. Appl. Phys. 98, 093714 (2005). [9] N. Miyashita, Y. Shimizu, and Y. Okada, J. Appl. Phys. 102, 044904 (2007). [10] G. M. Peake, K. E. Waldrip, T. W. Hargett, N. A. Modine, and D. K. Serkland, J. Cryst. Growth 261, 398 (2004). [11] S. Adachi, Physical Properties of III–V Semiconductor Compounds: InP, InAs, GaAs, GaP, InGaAs, and InGaAsP, John Wiley & Sons Ltd, New York, 1992. [12] Y. Liu, H. Jiang, T. Egawa, B. Zhang, and H. Ishikawa, J. Appl. Phys. 99, 123702 (2006). [13] M. Sotoodeh, A. H. Khalid, and A. A. Rezazadeh, J. Appl. Phys. 87, 2890 (2000). [14] T. Hofmann, G. Leibiger, V. Gottschalch, I. Pietzonka, and M. Schubert, Phys. Rev. B 64, 155206 (2001). [15] Z. P. Wei, B. Yao, Z. Z. Zhang, Y. M. Lu, D. Z. Shen, B. H. Li, X. H. Wang, J. Y. Zhang, D. X. Zhao, X. W. Fan, and Z. K. Tang, Appl. Phys. Lett. 89, 102104 (2006). [16] K. Perzynska, F. Firszt, S. Ł e˛ gowski, H. Meczy ˛ nska, J. Szatkowski, M. Biernacka, A. Gajlewicz, S. Tarasenko, and P. Zaleski, J. Cryst. Growth 214/215 904 (2000). [17] W. Dobrowolski, R. R. Gał˛a zka, E. Grodzicka, J. Kossut, and B. Witkowska, Phys. Rev. B 48, 17848 (1993). [18] J. C. Erickson, H. W. Yao, R. B. James, H. Hermon, and M. Greaves, J. Electron. Mater. 29, 699 (2000). [19] R. W. Miles, in Properties of Narrow Gap Cadmiun-based Compounds, EMIS Datareviews Series No. 10 (edited by P. Capper), INSPEC, London, 1994, p. 221. [20] A. F. M. Anwar, S. Wu, and R. T. Webster, IEEE Trans. Electron Dev. 48, 567 (2001). [21] E. Bellotti, F. Bertazzi, and M. Goano, J. Appl. Phys. 101, 123706 (2007). [22] R. Sakamoto, K. Nakata, and S. Nakajima, Physica B 272, 250 (1999). [23] M. Yee, P. A. Houston, and J. P. R. David, J. Appl. Phys. 91, 1601 (2002). [24] P. K. Bhattacharya, U. Das, and M. J. Ludowise, Phys. Rev. B 29, 6623 (1984). [25] K. Brennan and K. Hess, J. Appl. Phys. 59, 964 (1986). [26] V. Balynas, A. Krotkus, A. Stalnionis, A. T. Gorelionok, N. M. Shmidt, and J. A. Tellefsen, Appl. Phys. A 51, 357 (1990). [27] D. Hahn and A. Schlachetzki, J. Electron. Mater. 21, 1147 (1992).

CARRIER TRANSPORT PROPERTIES

387

[28] A. Patane, A. Ignatov, D. Fowler, O. Makarovsky, L. Eaves, L. Geelhaar, and H. Riechert, Phys. Rev. B 72, 033312 (2005). [29] J. -S. Rieh, P. K. Bhattacharya, and E. T. Croke, IEEE Trans. Electron Dev. 47, 883 (2000). [30] S. Adachi, Handbook on Physical Properties of Semiconductors: Volume 1 Group IV Semiconductors, Kluwer Academic, Boston, 2004. [31] S. Chakraborty, M. K. Bera, S. Bhattacharya, P. K. Bose, and C. K. Maiti, Thin Solid Films 504, 73 (2006). [32] A. G. Ulyashin, N. V. Abrosimov, A. Bentzen, A. Suphellen, E. Sauar, and B. G. Svensson, Mater. Sci. Semicond. Process. 9, 772 (2006). [33] R. Shivaram, G. Niu, J. D. Cressler, and E. T. Croke, Solid-State Electron. 44, 559 (2000). [34] S. K. Samanta, S. Maikap, S. Chatterjee, and C. K. Maiti, Solid-State Electron. 47, 893 (2003). [35] M. S. Carroll and C. A. King, J. Appl. Phys. 93, 1656 (2003). [36] I. Z. Mitrovic, O. Buiu, S. Hall, J. Zhang, Y. Wang, P. L. F. Hemment, H. A. W. El Mubarek, and P. Ashburn, Semicond. Sci. Technol. 20, 95 (2005). [37] A. Cremades, M. Albrecht, J. Krinke, R. Dimitrov, M. Stutzmann, and H. P. Strunk, J. Appl. Phys. 87, 2357 (2000). [38] K. Kumakura, T. Makimoto, N. Kobayashi, T. Hashizume, T. Fukui, and H. Hasegawa, J. Cryst. Growth 298, 787 (2007). [39] B. F. Levine, W. T. Tsang, C. G. Bethea, and F. Capasso, Appl. Phys. Lett. 41, 470 (1982). [40] B. F. Levine, C. G. Bethea, W. T. Tsang, F. Capasso, K. K. Thornber, R. C. Fulton, and D. A. Kleinman, Appl. Phys. Lett. 42, 769 (1983). [41] R. K. Ahrenkiel, in Properties of Aluminium Gallium Arsenide, EMIS Datareviews Series No. 7 (edited by S. Adachi), INSPEC, London, 1993, p. 221. [42] R. A. J. Thomeer, P. R. Hageman, and L. J. Giling, Appl. Phys. Lett. 64, 1561 (1994). [43] J. Degani, R. F. Leheny, R. E. Nahory, and J. P. Heritage, Appl. Phys. Lett. 39, 569 (1981). [44] P. Hill, J. Schlafer, W. Powazinik, E. Eichen, and R. Olshansky, Appl. Phys. Lett. 50, 1260 (1987). [45] N. Chand, in Properties of Lattice-matched and Strained Indium Gallium Arsenide, EMIS Datareviews Series No. 8 (edited by P. Bhattacharya), INSPEC, London, 1993, p. 127. [46] D. Vignaud, D. A. Yarekha, J. F. Lampin, M. Zaknoune, S. Godey, and F. Mollot, Appl. Phys. Lett. 90, 242104 (2007). [47] R. E. Welser, R. S. Setzko, K. S. Stevens, E. M. Rehder, C. R. Lutz, D. S. Hill, and P. J. Zampardi, J. Phys. Condens. Matter 16, S3373 (2004). [48] S. Sakai, M. Umeno, and Y. Amemiya, Jpn. J. Appl. Phys. 19, 109 (1980). [49] M. M. Tashima, L. W. Cook, and G. E. Stillman, J. Electron. Mater. 11, 831 (1982). [50] C. H. Henry, B. F. Levine, R. A. Logan, and C. G. Bethea, IEEE J. Quantum. Electron. QE-19, 905 (1983). [51] J. M. Borrego, S. Saroop, R. J. Gutmann, G. W. Charache, T. Donovan, P. F. Baldasaro, and C. A. Wang, J. Appl. Phys. 89, 3753 (2001). [52] D. Donetsky, S. Anikeev, G. Belenky, S. Luryi, C. A. Wang, and G. Nichols, Appl. Phys. Lett. 81, 4769 (2002). [53] S. Anikeev, D. Donetsky, G. Belenky, S. Luryi, C. A. Wang, J. M. Borrego, and G. Nichols, Appl. Phys. Lett. 83, 3317 (2003). [54] C. A. Wang, D. A. Shiau, D. Donetsky, S. Anikeev, G. Belenky, and S. Luryi, Appl. Phys. Lett. 86, 101910 (2005). [55] T. N. Danilova, B. E. Zhurtanov, A. N. Imenkov, and Y. P. Yakovlev, Semicond. 39, 1235 (2005). [56] V. Bhagwat, Y. G. Xiao, I. Bhat, P. Dutta, T. F. Refaat, M. N. Abedin, and V. Kumar, J. Electron. Mater. 35, 1613 (2006). [57] S. A. Wood, C. H. Molloy, P. M. Smowton, P. Blood, and C. C. Button, IEEE J. Quantum Electron. 36, 742 (2000). [58] P. C. Mogensen, G. Jones, N. Cain, P. Blood, D. J. Mowbray, S. W. Bland, D. Peggs, and R. P. Petrie, Inst. Phys. Conf. Ser. 162, 161 (1999).

388

PROPERTIES OF SEMICONDUCTOR ALLOYS

[59] O. Lopatiuk, W. Burdett, L. Chernyak, K. P. Ip, Y. W. Heo, D. P. Norton, S. J. Pearton, B. Hertog, P. P. Chow, and A. Osinsky, Appl. Phys. Lett. 86, 012105 (2005). [60] P. Lemasson, A. Forveille-Boutry, and R. Triboulet, J. Appl. Phys. 55, 592 (1984). [61] J. Franc, P. H€oschl, E. Belas, R. Grill, P. Hlıdek, P. Moravec, and J. Bok, Nucl. Instrum. Methods Phys. Res. A 434, 146 (1999). [62] K. N. Oh, K. H. Kim, J. K. Hong, Y. C. Chung, S. U. Kim, and M. J. Park, J. Cryst. Growth 184, 1247 (1998). [63] P Capper, Y. Nemirovsky, R. Fastow, C. L. Jones, in Properties of Narrow Gap Cadmiun-based Compounds, EMIS Datareviews Series No. 10 (edited by P. Capper), INSPEC, London, 1994, pp. 227–241. [64] J. Lee, A. L. Gutierrez-Aitken, S. H. Li, and P. K. Bhattacharya, IEEE Trans. Electron Dev. 43, 977 (1996). [65] K. Yeom, J. M. Hinckley, and J. Singh, J. Appl. Phys. 80, 6773 (1996). [66] K. Kunihiro, K. Kasahara, Y. Takahashi, and Y. Ohno, IEEE Electron Dev. Lett. 20, 608 (1999). [67] T. Tut, M. Gokkavas, B. Butun, S. Butun, E. Ulker, and E. Ozbay, Appl. Phys. Lett. 89, 183524 (2006). [68] S. -L. Fu, T. P. Chin, M. C. Ho, C. W. Tu, and P. M. Asbeck, Appl. Phys. Lett. 66, 3507 (1995). [69] R. Ghin, J. P. R. David, S. A. Plimmer, M. Hopkinson, G. J. Rees, D. C. Herbert, and D. R. Wight, IEEE Trans. Electron Dev. 45, 2096 (1998). [70] C. K. Chia, J. P. R. David, G. J. Rees, S. A. Plimmer, R. Grey, and P. N. Robson, J. Appl. Phys. 84, 4363 (1998). [71] S. A. Plimmer, J. P. R. David, R. Grey, and G. J. Rees, IEEE Trans. Electron Dev. 47, 1089 (2000). [72] X. G. Zheng, P. Yuan, X. Sun, G. S. Kinsey, A. L. Holmes, B. G. Streetman, and J. C. Campbell, IEEE J. Quantum Electron. 36, 1168 (2000). [73] B. K. Ng, J. P. R. David, G. J. Rees, R. C. Tozer, M. Hopkinson, and R. J. Airey, IEEE Trans. Electron Dev. 49, 2349 (2002). [74] Y. L. Goh, A. R. J. Marshall, D. J. Massey, J. S. Ng, C. H. Tan, M. Hopkinson, J. P. R. David, S. K. Jones, C. C. Button, and S. M. Pinches, IEEE J. Quantum Electron. 43, 503 (2007). [75] D. Ritter, R. A. Hamm, A. Feygenson, and M. B. Panish, Appl. Phys. Lett. 60, 3150 (1992). [76] R. J. Malik, N. Chand, J. Nagle, R. W. Ryan, K. Alavi, and A. Y. Cho, IEEE Electron Dev. Lett. 13, 557 (1992). [77] A. Neviani, G. Meneghesso, E. Zanoni, M. Hafizi, and C. Canali, IEEE Electron Dev. Lett. 18, 619 (1997). [78] M. Yee, J. P. R. David, P. A. Houston, C. H. Tan, and A. Krysa, IEEE Trans. Electron Dev. 50, 2021 (2003). [79] W. K. Ng, C. H. Tan, J. P. R. David, P. A. Houston, M. Yee, and J. S. Ng, Appl. Phys. Lett. 83, 2820 (2003). [80] J. Bude and K. Hess, J. Appl. Phys. 72, 3554 (1992). [81] M. Isler, Phys. Rev. B 63, 115209 (2001). [82] C. H. Tan, G. J. Rees, P. A. Houston, J. S. Ng, W. K. Ng, and J. P. R. David, Appl. Phys. Lett. 84, 2322 (2004). [83] K. Y. Choo and D. S. Ong, J. Appl. Phys. 98, 023714 (2005). [84] J. S. Ng, C. H. Tan, J. P. R. David, G. Hill, and G. J. Rees, IEEE Trans. Electron Dev. 50, 901 (2003). [85] Y. C. Chen and P. K. Bhattacharya, J. Appl. Phys. 73, 465 (1993). [86] O. Hildebrand, W. Kuebart, and M. H. Pilkuhn, Appl. Phys. Lett. 37, 801 (1980). [87] M. Z. Zhingarev, V. I. Korolkov, M. P. Mikhailova, and V. V. Sazonov, Sov. Tech. Phys. Lett. 7, 637 (1981). [88] H. Kuwatsuka, T. Mikawa, S. Miura, N. Yasuoka, M. Ito, T. Tanahashi, and O. Wada, J. Appl. Phys. 70, 2169 (1991). [89] L. Gouskov, B. Orsal, M. Perotin, M. Karim, A. Sabir, P. Coudray, S. Kibeya, and H. Luquet, Appl. Phys. Lett. 60, 3030 (1992).

CARRIER TRANSPORT PROPERTIES

389

[90] A. Rmou, H. Luquet, L. Gouskov, M. Perotin, and P. Coudray, Jpn. J. Appl. Phys. 33, 4657 (1994). [91] G. S. Kinsey, D. W. Gotthold, A. L. Holmes, Jr., B. G. Streetman, and J. C. Campbell, Appl. Phys. Lett. 76, 2824 (2000). [92] V. M. Andreev, M. Z. Zhingarev, O. O. Iventeva, V. I. Korolkov, and M. P. Mikhaılova, Sov. Phys. Semicond. 15, 701 (1981). [93] B. A. Matveev, M. P. Mikhaılova, S. V. Slobodchikov, N. N. Smirnova, N. M. Stus, and G. N. Talalakin, Sov. Phys. Semicond. 13, 294 (1979). [94] F. Osaka, T. Mikawa, and T. Kaneda, Appl. Phys. Lett. 46, 1138 (1985). [95] F. Osaka, T. Mikawa, and T. Kaneda, IEEE J. Quantum Electron. QE-21, 1326 (1985). [96] N. Shamir and D. Ritter, IEEE Trans. Electron Dev. 47, 488 (2000). [97] N. Shamir and D. Ritter, IEEE Electron Dev. Lett. 21, 509 (2000). [98] I. A. Andreev, M. P. Mikhaılova, S. V. Melnikov, Y. P. Smorchkova, and Y. P. Yakovlev, Sov. Phys. Semicond. 25, 861 (1991). [99] M. Tsuji, K. Makita, I. Watanabe, and K. Taguchi, Appl. Phys. Lett. 65, 3248 (1994). [100] K. F. Brennan and N. S. Mansour, J. Appl. Phys. 69, 7844 (1991).

Index Page numbers in italic refer to figures or tables. Alloys are listed according to elemental composition. Abeles’s model 63–4 AlAsSb band-gap energies 174–5 optical properties 323 phonon frequencies 108 thermal conductivity 70 AlGaAs band offsets GaAs interface 278–9 GaInP interface 278 band-gap energies 157–60 deformation potential 263–4, 269–70, 271–2 effective masses 239–41 elastic properties 90, 96 electro-optic constant 358, 359 Franz–Keldysh effect 360 impact ionization coefficient 383 low-field mobility 369, 377–8 microhardness 93 minority-carrier transport 380–1 nonlinear optical constant 361–2 optical properties 316, 317 phonon frequencies 106–7, 113–15, 120 photoelastic constant 357, 358 piezoelectric constant 128–9 thermal conductivity 68, 69 thermal diffusivity 75–6 AlGaAsSb band offsets GaInAsSb interface 282 InP/InAs/GaSb interfaces 281 band-gap energies 187–8, 196 optical properties 328 Schottky barrier 296–7 AlGaIn and coherent epitaxy 37 phonon frequencies 108, 109

AlGaInAs band offsets, GaInAs interface 283 band-gap energies 194–5 effective masses 250, 251 impact ionization coefficient 385 optical properties 331–2 Schottky barrier 298–9 thermal conductivity 74 AlGaInN crystal lattice parameters 25, 26 low-field mobility 373–4 Schottky barrier 297–8 thermal conductivity 68, 69, 70 AlGaInP band offsets AlInP interface 282 GaInP interface 282–3 band-gap energies 187, 191, 193–4, 196 effective masses 250 elastic properties 81, 86 low-field mobility 373–4 minority-carrier transport 382 optical properties 330–1 Schottky barrier 298 thermal conductivity 74 AlGaN band offsets, GaN interface 283–4 band-gap energies 149–51 and critical thickness 38 deformation potential 261–2, 263 impact ionization coefficient 382 low-field mobility 368, 376, 377 minority-carrier transport 380 nonlinear optical constant 361 optical properties 311–12 phonon frequencies 105–6 piezoelectric constant 125 Schottky barrier 291

Properties of Semiconductor Alloys: Group-IV, III–V and II–VI Semiconductors © 2009 John Wiley & Sons, Ltd. ISBN: 978-0-470-74369-0

Sadao Adachi

392

INDEX

AlGaNAs band-gap energies 184–5 optical properties 326–7 AlGaP band-gap energies 153, 154 effective masses 238–9 optical properties 314 AlGaPAs band-gap energies 186–7 optical properties 326–7 AlGaSb band-gap energies 163–5 effective masses 242–3 impact ionization coefficient 384 lattice parameters 26, 27 low-field mobility 369–70 Schottky barrier 294–5 AlInAs band offsets GaInAS interface 280 InP interface 279 band-gap energies 160–1 deformation potential 264 effective masses 240, 241 elastic properties 89, 90 optical properties 316–17, 318 Schottky barrier 293–4 AlInAsSb band offsets, GaInAsSb interface 282 band-gap energies 187, 188–9, 196 AlInN band offsets, GaN interface 284 band-gap energies 150, 152 low-field mobility 368–9 optical properties 313, 314 AlInP band offsets AlGaInP interface 282 GaInP interface 277–8 band-gap energies 153–5 deformation potential 262–3 effective masses 238–9, 240 optical properties 314–15 AlInSb band-gap energies 165–6 effective masses 242–3 low-field mobility 369–70 optical properties 319, 320 alloy scattering 365 alloys defined and described 1

AlPAs band-gap energies 174–5 effective masses 245 AlPSb band-gap energies 174–5 effective masses 245 optical properties 322 Au/GaInP rectifiers 292 band offsets see heterojunction band offsets band-gap energies background and theory bowing parameter 136 interpolation of parameters 4–7 ordered/disordered alloy 136–9 quasi-cubic band model 133–6, 135 group IV alloys binary 139–45 ternary 145–7, 149 III-V ternary alloys Al–(V, V) 174–5 Ga–(V, V) 175–9 In–(V, V) 179–84 dilute-nitride III–(V, V) 166–74 (III, III)–As 157–63 (III, III)–N 149–53 (III, III)–P 153–7 (III, III)–Sb 163–6 summary 183–4 III–V quaternary alloys dilute-nitride 184–93 (III, III, III)–V 193–5 III–(V, V, V) 195 summary 196–7 II–VI ternary alloys Cd–(VI, VI) 210–12 Zn–(VI, VI) 208–10 (II, II)–O 197–8 (II, II)–S 198–201 (II, II)–Se 201–4 (II, II)–Te 204–8 summary 214–16 II–VI quaternary alloys (II, II, II)–VI 213–14 (II, II)–(VI, VI) 212–13 summary 214–16 BeCdSe band-gap energies 199, 201, 202 optical properties 335 BeCdTe, band-gap energies 199, 201, 202 BeMgCdSe, band-gap energies 213–14

INDEX BeMgZnSe band offsets, ZnSe interface 289 band-gap energies 213, 214 optical properties 346 BeS/BeSe/BeTe, elastic properties 90–1, 93–4 BeZnCdSe, optical properties 346 BeZnO band-gap energies 197, 198, 199, 215 optical properties 332 BeZnSe band offsets, ZnSe interface 287–8 band-gap energies 199, 201–2 elastic properties 84–5, 86, 94 optical properties 335, 336 phonon frequencies 111, 118 photoelastic constant 357 BeZnTe band-energies 199, 201–2, 215 band-gap energies 199, 204–5 optical properties 339 phonon frequencies 111 bilayer model 34–5 binary mixed valence compounds 2–4 bond distances 21 bowing parameters 5, 6, 7, 136 dilute-nitride III–V alloys 167 electron and hole mobilities 367 III–V ternaries 184 II–VI ternaries 215 Brillouin scattering 357 carrier transport properties 365–7 high-field mobility 376–9 impact ionization coefficient 382–6 low-field mobility 367–76 minority-carrier transport 379–82 CdHgS, band-gap energies 199, 200–1 CdHgSe band-gap energies 199, 201, 203–4, 215 low-field mobility 374 optical properties 338–9 CdHgTe band offsets, CdTe interface 288–9 band-gap energies 199, 208, 215 Debye temperature 58–9 effective masses 252, 254 Frank–Keldysh effect 361 impact ionization coefficient 386 low-field mobility 375 minority-carrier transport 382 nonlinear optical constant 362

393

optical properties 342 phonon frequencies 109, 111 specific heat 56 thermal conductivity 74–5 thermal expansion coefficient 63 CdSeTe band-gap energies 211–12 optical properties 346 phase diagram 50 CdSSe band-gap energies 210–11 effective masses 253 electro-optic constant 359–60 Franz–Keldysh effect 360–1 optical properties 344–5 CdSTe band-gap energies 211 lattice parameters 31 optical properties 345 phase diagram 49–50 CGe band-gap energies 140–1, 147, 149 optical properties 309 chalcopyrite structures 14 cleavage plane 41 coherent epitaxy bilayer model 32–3 critical thickness 37–9 elastic strain and lattice deformation 33–7 lattice-mismatch of dilute-nitrides 167–8 compliance constants 81, 82–3 composite structures see coherent epitaxy compound semiconductors 1, 10 conduction band structure 133, 134 critical thickness 37–9 crystal density calculation 22 data 18, 19 crystal structure 2 lattice constant/parameters 15–31 random alloy 11 spontaneous ordering 11–15 CSi band offsets Si interface 276–7 SiGe interface 277 band-gap energies 139–40, 147–9 Debye temperature 57–8 effective masses 234–7 elastic properties 89 electro-optic constant 358

394

INDEX

CSi (Continued) Fr€ohlich coupling constant 130 lattice mismatch in epilayers 35–6 low-field mobility 367 microhardness 92 optical properties 308–9 piezoelectric constant 125, 127 thermal conductivity 66, 67 thermal diffusivity 75–6 CSiGe band offsets, Si interface 276–7 band-gap energies 145–7 minority-carrier transport 380 optical properties 311 Schottky barrier 291 CuAu elastic properties 82 electrical resistivity 365, 366 lattice constant 15–16 thermal resistivity 65–6, 365, 366 CuAu-I structure 12, 14, 15, 66 CuPt-B structure 12, 14, 15 energy-band diagram 136, 137 Debye temperature 52–3, 56–7 group IV alloy 57–8 III–V alloy 58 II–VI alloy 58–9 deformation potential (intervalley) group IV alloy 270–1 III–V alloy 271–2 deformation potential (intravalley) group IV alloy 259–61 high-symmetry points 267–9 III–V ternary alloy 261–6 high-symmetry points 269–70 III–V quaternary alloy 266 II–VI quaternary alloy 266–7 deformation potential (phonon) 121–3 density-of-state effective mass 229, 232 diamond structure 21 dielectric constants 308 dispersion 307 drift velocities 365 effective masses background and theory compositional dependence 254 electron effective mass 229–30, 231 hole effective mass 230–2, 233, 234, 235, 236

interpolation scheme 232–4 temperature and pressure dependence 254–6 group IV binary alloys 234–8 III–V ternary alloys Al–(V, V) 245, 246 Ga–(V, V) 245–6 In–(V, V) 246–7 dilute-nitride III–(V, V) 243–5 (III, III)–As 239–42 (III, III)–N 238, 239 (III, III)–P 238–9 (III, III)–Sb 242–3 III–V quaternary alloys dilute-nitride 248 (III, III, III)–V 250–1 (III, III)–(V, V) 248–50 II–VI ternary alloys (II, II)–VI 251–3 II–(VI, VI) 253 II–VI quaternary alloys (II, II)–(VI, VI) 253–4 elastic constants 81, 82–3 group IV alloy 81 III–V alloy 81, 83–4 II–VI 84–6 pressure effect 88 and sound velocity 96–7 temperature effect 86–8 third-order constant 39 see also Young’s modulus elastic strain 33–7 elasto-optic effect 357–8 electrical resistivity 365, 366 electro-optic constants linear 358–60 quadratic 360–1 electron mobility See low-field mobility; minority-carrier transport elemental semiconductors 1, 2 energy-band structure see band-gap energies; effective masses epitaxy see coherent epitaxy Franz–Keldysh effect 360–1 Fr€ ohlich coupling constant 129–31 GaAsIn, phase diagram 46, 47 GaAsInP specific heat 55 thermal conductivity and diffusivity 75–6

INDEX GaAsSb band-gap energies 178–9 effective masses 246 impact ionization coefficient 385 optical properties 324 phonon frequencies 100, 108 Schottky barrier 295–6 thermal conductivity 73 GaInAs band offsets AlGaInAs interface 283 AlInAS interface 280 GaAs interface 284–6 GaN interface 284 InP interface 279–80 band-gap energies 161, 163 deformation potential 265 effective masses 240, 241–2, 256 elastic properties 89, 90 impact ionization coefficient 383–4 low-field mobility 377–8 near neighbour distances 28 optical properties 318–19 phase diagram 46, 47 piezoelectric constant 128 Schottky barrier 294 thermal conductivity 68, 69, 70 GaInAsSb band offsets AlGaAsSb interface 282 AlInAsSb interface 282 GaSb/InP/InAs interfaces 281 band-gap energies 196 effective masses 249–50 optical properties 328–30 Schottky barrier 296–7 thermal conductivity 70, 71, 72 GaInN band offsets, GaN interface 284 band-gap energies 150, 151, 152–3 and critical thickness 38 deformation potential 262, 263 low-field mobility 368, 376, 377 near neighbour distances 28, 29 optical properties 313–14 phase diagram 47–8 phonon frequencies 105–6 piezoelectric constant 126–8 thermal conductivity 68, 69, 70 GaInNAs band offsets, GaAs interface 286–7

band-gap energies 166–7, 168, 185 effective masses 248, 254, 256 optical properties 326 GaInNP band-gap energies 185 optical properties 326 GaInP band offsets AlGaInP interface 282–3 AlInP interface 277–8 GaAs interface 277 band-gap energies 137–9, 155–7 deformation potential 263 effective masses 239, 240 elastic properties 89, 90 Franz–Keldysh effect 360 impact ionization coefficient 383 low-field mobility 369 nonlinear optical constant 362 optical properties 315–16 phonon frequencies 100, 108, 115 photoelastic constant 357 Schottky barrier 292 thermal conductivity 73 GaInPAs band offsets, InP interface 280–1 band-gap energies 187, 189–91, 196–7 and coherent epitaxy 34–5, 38 deformation potential 266, 267 effective masses 248–9, 256 elastic properties 81, 86, 87, 88, 96 Fr€ ohlich coupling constant 131 impact ionization coefficient 385 low-field mobility 372–3, 378–9 microhardness 92–3, 94 minority-carrier transport 381–2 near neighbour distances 28, 29 phonon frequencies 108 piezoelectric constant 128–9 Schottky barrier 296 thermal conductivity 70, 71, 72 GaInPSb, minority-carrier transport 381–2 GaInSb band-gap energies 166, 167, 168 effective masses 242–3 elastic properties 81, 83, 85 microhardness 93 minority-carrier transport 381 optical properties 319, 320 phase diagram 46, 47 phase transition 40–1

395

396

INDEX

GaInSb (Continued) phonon frequencies 107, 108 Schottky barrier 294–5 thermal conductivity 68, 69, 70 GaNAs band offsets, GaAs interface 286 band-gap energies 166–7, 168, 171–2 and coherent epitaxy 36 deformation potential 265–6 effective masses 243–4 impact ionization coefficient 384 low-field mobility 371, 378 mode Gr€uneisen parameter 121 optical properties 321, 322 GaNAsSb, band offsets, GaAs interface 287 GaNP effective masses 243 optical properties 320–1 GaNP, band-gap energies 170–1 GaNPAs, band-gap energies 185–6 GaNSb band-gap energies 172 optical properties 321 GaPAs band-gap energies 175–6 deformation potentials 263–4, 266, 269–70 effective masses 245, 246 low-field mobility 371, 372 optical properties 323–4 phonon frequencies 108, 115, 116, 122–3 GaPSb band-gap energies 176–7 optical properties 324 Schottky barrier 295 GaSbAs, low-field mobility 371, 372 GeSn band-gap energies 144–5, 147, 148 optical properties 309–10 Grimm–Sommerfeld rule 2–4 Gr€uneisen parameter 119–21 phonon deformation potential 121–3 Hall mobilities 366, 367 heterojunction band offsets 275 group IV systems 275–7 III–V lattice matched system ternary alloy 277–80 quaternary alloy 280–3 III–V lattice mis-matched system II–V systems 287–9

283–7

HgSeTe, phase diagram 51 high-field transport group IV 376 III–V ternary alloys dilute-nitride III–(V, V) 378 (III, III)–As 377–8 (III, III)–N 376 (III, III)–P 376–7 III–V quaternary alloys 378–9 II–IV alloys 379 high-frequency dielectric constant 308 hole effective mass 230–2, 233, 234, 235, 236 hole mobilities 366, 367 impact ionization coefficient group IV alloys 382 III–V ternary alloys dilute-nitride III–(V, V) 384–5 Ga–(V, V) 385 In–(V, V) 385 (III, III)–As 383–4 (III, III)–N 382–3 (III, III)–P 383 (III, III)–Sb 384 III–V quaternary alloys (III, III, III)–V 385 (III, III)–(V, V) 385 II–VI 386 InAsSb band offsets, GaSb interface 280 band-gap energies 181–3 effective masses 247 impact ionization coefficient 385 low-field mobility 371, 372 optical properties 325 InGaAs, Fr€ ohlich coupling 129 InNAs band-gap energies 173 effective masses 244–5 low-field mobility 371 InNP band-gap energies 173 optical properties 322 InNSb band-gap energies 174 effective masses 245 InPAs band-gap energies 179, 180 Debye temperature 58 effective masses 246–7, 255, 256

INDEX low-field mobility 371, 372 optical properties 324–5 specific heat 54, 55 thermal conductivity 70, 71 InPAsSb band-gap energies 195, 196 effective masses 250–1 InPSb band-gap energies 179–81 low-field mobility 371, 372 optical properties 325 interpolation schemes band-gap 4–7 effective masses 232–4 intravalley/intervalley deformation potential see deformation potential ionicity 9, 10 isotopic abundance 9 lattice constants/parameters Cu–Au alloy 15–16 group IV semiconductor 19–22 III–V semiconductor 22–9 II–VI semiconductor 29–31 non-alloyed semiconductors 16–19 lattice strain/deformation/mismatch see coherent epitaxy lattice-matching data 22, 23, 24, 30 linear electro-optic constant 358–60 long-wavelength phonon see phonon low-field mobility 366, 367 group IV binary alloys 367–8 III–V ternary alloys dilute-nitride III–(V, V) 370 Ga–(V, V) 371 In–(V, V) 371 (III–III)–As 369 (III–III)–N 368–9 (III–III)–P 369 (III–III)–Sb 369–70 III–V quaternary alloys dilute-nitride 371–2 (III, III, III)–V 373–4 (III, III)–(V, V) 372–3 II–VI ternary alloys Zn–(V, V) 375 (II, II)–O 374 (II, II)–Se 374–5 (II, II)–Te 375 Luttinger’s parameters 231, 233, 234

Matthews–Blakeslee theory 38 melting points 51, 52–3 see also phase diagrams MgCdSe band-gap energies 199, 201, 202–3, 215 low-field mobility 374–5 optical properties 337 MgCdTe band-gap energies 199, 206, 215 optical properties 340 MgZnCdSe band offsets, ZnCdSe interface 289 band-gap energies 214 optical properties 346–7 MgZnO band offsets, CdS interface 287 band-gap energies 197–8, 199, 215 and coherent epitaxy 37 deformation potential 267 effective masses 251–2 low-field mobility 374 minority-carrier transport 382 optical properties 332–3 phase diagram 48–9 MgZnS band-gap energies 198–9, 205 optical properties 333–4 MgZnSe band offsets ZnCdSe interface 289 ZnSe interface 287–8 band-gap energies 199, 201, 202, 215 low-field mobility 374–5 nonlinear optical constant 362 optical properties 335–7 thermal expansion coefficient 63 MgZnSeTe optical properties 346 phonon frequencies 112 MgZnSSe band offsets, ZnSe interface 289 bang-gap energies 212–13 effective masses 253–4 optical properties 346 phonon frequencies 111–12 MgZnSTe, band-gap energies 212, 213 MgZnTe band-gap energies 199, 205–6, 215 optical properties 339–40 Schottky barrier 299

397

398

INDEX

microhardness group IV alloy 92 III–V alloy 92–3 II–VI alloy 93–6 minority–carrier transport group IV alloys binary 379–80 ternary 380 III–V ternary alloys (III, III)–Ga 381 (III, III)–N 380 III–V quaternary alloys (III, III, III)–V 382 (III, III)–(V, V) 381–2 II–IV alloys 382 mode Gr€uneisen see Gr€uneisen parameter molecular weight calculating 9–10 non-alloyed semiconductor data 18, 19 multilayer structures see coherent epitaxy nonlinear optical constant

361–2

optical properties dielectric constants 308 dispersion relations 307 group IV alloys binary 308–11 ternary 311 III–V ternary alloys Al–(V, V) 322–3 Ga–(V, V) 323–4 In–(V, V) 324–6 dilute-nitride III–(V, V) 320–2 (III, III)–As 316–20 (III, III)–N 311–14 (III, III)–P 314–16 III–V quaternary alloys dilute-nitride 326 (III, III, III)–V 330–2 (III, III)–(V, V) 326–30 III–(V, V, V) 332 II–VI ternary alloys Cd–(VI, VI) 344–6 Zn–(VI, VI) 343–4 (II, II)–O 332–3 (II, II)–S 333–5 (II, II)–Se 335–9 (II, II)–Te 339–42 II–VI quaternary alloys (II, II, II )–VI 346–7

(II, II)–(VI, VI) 346 see also elasto-optic; electro-optic ordering see spontaneous ordering periodic table 2 phase diagrams group IV alloys 45 III–V alloys 45–8 II–VI alloys 48–51 phase transition, structural 39–41 Phillips ionicity 9, 10 phonon frequencies/modes 99–100, 101, 102, 104–5, 110 group IV alloy 100–4, 112–13 III–V alloy 104–9, 113–15 II–VI alloy 109–12, 115–19 mode Gr€ uneisen parameter 119–21 phonon deformation potential 121–3 temperature and pressure dependence 112–19 photoelastic coefficient 357–8 piezoelectric semiconductors 97, 126 stress and strain constants 125–9 pseudomorphic epitaxy 37–9 quadratic electro-optic constant

360–1

reflectivity 307 refractive index 307 resistivity electrical 365, 366 thermal 64, 65, 67, 68, 365, 366 Schottky barrier 289–90 group IV alloys 290–1 III–V ternary alloys Ga–(V, V) 295–6 (III, III)–As 292–4 (III, III)–N 291 (III, III)–P 292 (III, III)–Sb 294–5 III–V quaternary alloys (III, III, III)–V 297–9 (III, III)–(V, V) 296–7 II–VI ternary alloys Zn–(VI, VI) 300 (II, II)–Te 299 semiconductor types 1 SiC 1, 2 Franz–Keldysh effect 360 phonon frequencies 100, 102

INDEX SiGe band offsets, Si interface 276 band-gap energies 148 relaxed alloy 141–3 strained alloy 143–4 and critical thickness 38, 39 crystal lattice parameters 19–22 deformation potential 259–61, 269 effective masses 237–8 elastic properties 81, 84, 85 electro-optic constant 358 Fr€ohlich coupling constant 130 impact ionization coefficient 382, 383 low-field mobility 367–8 minority-carrier transport 379–80 optical properties 309–10 ordered structures 12, 13–14 phase diagram 45, 46 phonon frequencies 100–4, 113, 121–2 Schottky barrier 290–1 specific heat 53–4 thermal conductivity 66, 68 SiGeSn, band gap energies 147 SiSn, band gap energies 148–9 sound velocity 96–7 specific heat group IV alloys 51, 52–3, 53–4 III–V alloys 54–5 II–VI alloys 55 spontaneous ordering energy-band gaps 136–9 group IV alloy 11, 12 III-V alloy 12, 14–15 II–VI alloy 12, 15 structural phase transition 39–41 surface energy 41 tetrahedral rule 3–4 thermal conductivity 52–3, 63–6, 67 group IV alloy 66–8 III–V alloy 68–74 II–VI alloy 74–5 thermal diffusivity 75–6 thermal expansion coefficient 52–3 group IV alloys 59–61 III–V alloys 61–3 II–VI alloys 63 thermal resistivity 64, 65, 67, 68, 365, 366 thin films see critical thickness transport see carrier transport

399

valence band structure 133, 134 valence binary compounds 3–4 valence electrons 2–3 Varshni parameters 159–60, 163 Vegard law 20, 25–6, 28, 36, 37, 57, 141 Wiedemann–Franz law 65, 365 wurtxite structure 21 Young’s modulus group IV alloy 89 III–V alloy 89–90 II–VI alloy 90–2 zinc blende structure 21 energy band diagram 136, 137 ZnCdO band-gap energies 198, 199, 215 optical properties 333 ZnCdS band offsets, ZnS interface 287 band-gap energies 199, 200, 215 deformation potential 267 nonlinear optical constant 362 optical properties 334–5 phase transition 40, 41 phonon frequencies 109, 111 ZnCdSe band offsets MgSSe interface 289 MgZnCdSe interface 289 MgZnSe interface 289 ZnSe interface 287–8 band-gap energies 199, 201, 203, 215 elastic properties 91–2 Franz–Keldysh effect 360–1 nonlinear optical constant 362 optical properties 337–8 phase transition 40, 41 phonon frequencies 109–11, 115–16, 118 ZnCdSSe, band offsets, ZnSSe interface 289 ZnCdTe band offsets CdTe interface 288 ZnTe interface 288 deformation potential 266–7 elastic properties 85, 87, 88 electro-optic constant 358–60 lattice parameters 29, 30, 31 phase diagram 49 low-field mobility 375

400

INDEX

ZnCdTe (Continued) nonlinear optical constant 361, 362 optical properties 340–1 phonon frequencies 109–11 photoelastic constant 357 Schottky barrier 299 structural phase transition 39, 40 ZnHgS, band-gap energies 199, 200, 215 ZnHgTe band-gap energies 199, 207–8 effective masses 252–3 microhardness 94–5 minority-carrier transport 382 optical properties 342 phonon frequencies 109 thermal conductivity 74 thermal expansion coefficient 63 ZnOS band-gap energies 208–9 optical properties 343

ZnOSe band-gap energies 209 deformation potential 267 ZnSeTe band-gap energies 209, 210 elastic properties 91–2, 94 low-field mobility 376 optical properties 344 phonon frequencies 118 ZnSSe band offsets, ZnSe/ZnCdSe interfaces band-gap energies 209–10 deformation potential 267 low-field mobility 376 optical properties 343 Schottky barrier 300 thermal expansion coefficient 63 ZnSTe band-gap energies 209, 210 deformation potential 267 optical properties 343–4

289

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close